SEL E C T E D
BY
G R E N O B L E
S C I E N C E S
Symmetry and Physical Properties of Crystals
C. Malgrange - C. Ric...

This content was uploaded by our users and we assume good faith they have the permission to share this book. If you own the copyright to this book and it is wrongfully on our website, we offer a simple DMCA procedure to remove your content from our site. Start by pressing the button below!

SEL E C T E D

BY

G R E N O B L E

S C I E N C E S

Symmetry and Physical Properties of Crystals

C. Malgrange - C. Ricolleau - M. Schlenker

Symmetry and Physical Properties of Crystals

Grenoble Sciences The aim of Grenoble Sciences is twofold: – to produce works corresponding to a clearly defined project, without the constraints of trends nor curriculum, – to ensure the utmost scientific and pedagogic quality of the selected works: each project is selected by Grenoble Sciences with the help of anonymous referees. In order to optimize the work, the authors interact for a year (on average) with the members of a reading committee, whose names figure in the front pages of the work, which is then co-published with the most suitable publishing partner. Contact: Tel.: (33) 4 76 51 46 95 E-mail: [email protected] Website: https://grenoble-sciences.ujf-grenoble.fr Scientific Director of Grenoble Sciences Jean Bornarel, Emeritus Professor at the Joseph Fourier University, Grenoble, France Grenoble Sciences is a department of the Joseph Fourier University supported by the ministère de l’Enseignement supérieur et de la Recherche and the région Rhône-Alpes. Symmetry and Physical Properties of Crystals is an improved version of the original book Symétrie et propriétés physiques des cristaux by Cécile Malgrange, Christian Ricolleau and Françoise Lefaucheux, EDP Sciences, Savoirs Actuels Series, 2011, ISBN 978 2 7598 0499 3. The Reading Committee included the following members: – Ryszard Cach, Professor, University of Wrocław (Wrocław, Poland) – Vladimir E. Dmitrienko, Chief Researcher, A.V. Shubnikov Institute of Crystallography (Moscow, Russia) – José Goulon, Emeritus CNRS Senior Researcher, former group leader at the European Synchrotron Radiation Facility (Grenoble, France) – Hiroo Hashizume, Emeritus Professor, Tokyo Institute of Technology (Tokyo, Japan) – Jochen Schneider, Professor, former DESY Research Director (Hamburg, Germany), former director of the Experimental Facilities Division for the LCLS (Stanford, USA) Translation from original French version performed by Michel Schlenker; typesetting: Stéphanie Trine—special thanks to Konstantin Protassov and Alexei Voronine; figures: Sylvie Bordage, Alain Jeanne-Michaud; cover illustration: Alice Giraud, with sample of pyrite: mineral collection of Pierre and Marie Curie University, photograph Jean-Pierre Boisseau

Cécile Malgrange Christian Ricolleau Michel Schlenker •

Symmetry and Physical Properties of Crystals

123

Cécile Malgrange Université Pierre et Marie Curie Institut de Minéralogie, de Physique des Matériaux et de Cosmochimie case 115, 4 place Jussieu 75252 Paris cedex 05 France

Michel Schlenker Université Grenoble-Alpes Grenoble-INP et Institut Néel du CNRS B.P. 166 38042 Grenoble cedex France

Christian Ricolleau Université Paris Diderot-Paris 7 Laboratoire Matériaux et Phénomènes Quantiques Bâtiment Condorcet, case 7021 75205 Paris cedex 13 France Translated, revised and adapted from ‘‘Symétrie et Propriétés Physiques des Cristaux’’, Cécile Malgrange, Christian Ricolleau et Françoise Lefaucheux, EDP Sciences/CNRS Éditions 2011

ISBN 978-94-017-8992-9 DOI 10.1007/978-94-017-8993-6

ISBN 978-94-017-8993-6

(eBook)

Library of Congress Control Number: 2014944543 Springer Dordrecht Heidelberg New York London Ó Springer Science+Business Media Dordrecht 2014 This work is subject to copyright. All rights are reserved by the Publisher, whether the whole or part of the material is concerned, specifically the rights of translation, reprinting, reuse of illustrations, recitation, broadcasting, reproduction on microfilms or in any other physical way, and transmission or information storage and retrieval, electronic adaptation, computer software, or by similar or dissimilar methodology now known or hereafter developed. Exempted from this legal reservation are brief excerpts in connection with reviews or scholarly analysis or material supplied specifically for the purpose of being entered and executed on a computer system, for exclusive use by the purchaser of the work. Duplication of this publication or parts thereof is permitted only under the provisions of the Copyright Law of the Publisher’s location, in its current version, and permission for use must always be obtained from Springer. Permissions for use may be obtained through RightsLink at the Copyright Clearance Center. Violations are liable to prosecution under the respective Copyright Law. The use of general descriptive names, registered names, trademarks, service marks, etc. in this publication does not imply, even in the absence of a specific statement, that such names are exempt from the relevant protective laws and regulations and therefore free for general use. While the advice and information in this book are believed to be true and accurate at the date of publication, neither the authors nor the editors nor the publisher can accept any legal responsibility for any errors or omissions that may be made. The publisher makes no warranty, express or implied, with respect to the material contained herein. Printed on acid-free paper Springer is part of Springer Science+Business Media (www.springer.com)

In memory of Hubert Curien (1924–2005), Professor at Pierre & Marie Curie University, Paris, and member of the French Academy of Sciences. A great administrator, Minister of Research in the French government, he shared his enthusiasm for crystallography with his students through the courses he gave throughout his career.

Foreword Apart from amorphous bodies such as glasses, the arrangement of ions, atoms and molecules in solid matter is regular and presents properties of symmetry. Crystals present both translational and orientational properties of symmetry, which govern their physical properties. It is because of their triple periodicity that crystals grow with a regular habit: quartz prisms, diamond octahedra or garnet rhomb-dodecahedra, and that they present planar cleavage faces, those of the cube for rock-salt, and those of the rhombohedron for Iceland spar. It is this same periodicity that is at the origin of the band structure of solids and conditions the properties of materials used in microelectronics. It is thanks to the redundancy of the information provided by the diﬀraction in phase of X-rays, neutrons or electrons, by all the molecular groups repeated by the translations of a crystal that one can determine their atomic structure. If one wishes to ﬁnd the structure of a complex molecule such as a protein or a virus, one should therefore crystallize it. This is done systematically during the elaboration of drugs by the pharmaceutical industry. The orientational symmetry of crystals is present in all their properties, ﬁrst of all in their external shape. But it is often because a particular element of symmetry is absent that a property may exist. It is because hydrated ammonium tartrate has no centre of symmetry that it is optically active, which Louis Pasteur associated to its external shape, right or left, thus discovering chirality (1848). It is because of symmetry considerations that the Curie brothers, Jacques and Pierre, looked for, and found, piezoelectricity in 1880. If one cools barium titanate below 120◦ C, its structure is modiﬁed. Above, it is cubic holohedral, below, it is tetragonal, with as its only symmetry elements a four-fold axis and mirrors parallel to that axis. It is this symmetry which makes it possible for a spontaneous electric polarisation to appear, and for the crystal to become pyroand ferroelectric. Generally speaking, the properties associated to structural phase changes depend on the relations between symmetry groups and their subgroups. The description of the symmetry operations of crystals and of the resulting physical properties is the aim of the present book. These operations are part of a complex system which was not grasped at once. It was a long way from Aristotle’s elements to the concept of space lattice. The ancients were always fascinated by the regularity of six-sided prisms of rock-crystal, as noted by

VIII

Symmetry and Physical Properties of Crystals

Pliny the Elder in his Natural History (77 A.D.). Kepler (1611), followed by Descartes (1637) and Bartholin (1661) tried to interpret the formation of sixcornered snowﬂakes by the agglomeration of six spherules round a seventh one. Kepler was the ﬁrst to describe the primitive and face-centred cubic lattices and the hexagonal lattice, although he did not call them that way. Compact pile-ups were considered similarly by Hooke (1665) and Huygens (1678) to explain the shape of quartz and the cleavage rhombohedron of calcite, respectively. The constancy of interfacial angles was established in the seventeenth and the eighteenth centuries by Steno (1669), Carangeot (1780) and Romé de l’Isle (1783). At the end of the eighteenth century, Bergman (1773) for calcite and Haüy (1784) in a general way, showed that the external shape of crystal may be obtained by a regular and triply periodic pile-up of identical elemental parallelepipeds, now called unit cells, and called molécules intégrantes by Haüy. But Haüy confused the unit cell with its chemical content and did not accept the notion of isomorphism introduced by Mitscherlich (1819). His classiﬁcation of crystals was based on their geometrical shape while that of the German School, led by Weiss (1817), was based on systems of symmetry axes. Haüy’s main merit was nevertheless to have introduced the notion of three-dimensional periodicity which deﬁnes the crystalline medium and to have established the geometrical properties of lattice planes by means of the law of simple rational intercepts. The relations between symmetry and properties were established in steps all along the nineteenth century: the 7 crystal systems (Mohs, 1822), the notion of point lattice (Seeber, 1824), the 32 crystal classes (Frankenheim, 1826; Hessel, 1830), the notion of hemihedry (Delafosse, 1840), molecular chirality (Pasteur, 1848), the 14 Bravais lattices (1850), groups of motion including helicoidal motions, the 65 chiral groups (Sohncke 1865), and, ﬁnally, the 230 space groups (Fedorov, 1890; Schoenﬂies, 1891; Barlow, 1894).1 The description of physical properties in their geometrical form requires in general other mathematical tools, such as tensors, which were ﬁrst introduced in elasticity by Voigt (1899) and Brillouin (1949). If one pulls a rod made of an isotropic material, its length increases and its cross-section decreases. A scalar is insuﬃcient to describe the response of the material to an excitation and two constants are necessary to describe the resulting deformation. Similarly, the polarisation of an anisotropic dielectric can only be expressed by way of a tensor. The book by Cécile Malgrange, Christian Ricolleau and Michel Schlenker is an extended translation of a ﬁrst version in French by Cécile Malgrange, Christian Ricolleau and Françoise Lefaucheux. It comprises three parts of roughly equal importance: 1) a ﬁrst part on crystal symmetry, symmetry operations, crystal lattices, point groups and space groups; 2) a second part on crystal anisotropy and tensors applied to elasticity, propagation of elastic waves in crystals and piezoelectricity; 3) a third one on the optical properties of crystals, polariza1. A. Authier, Early Days of X-Ray Crystallography (Oxford University Press, Oxford, 2013)

Foreword

IX

tion, optical activity and electro-optical eﬀects. The various types of chemical bonds are also described in a small chapter between the ﬁrst and the second parts. Most chapters include an annex on a particular topic related to one of the points developed in the chapter, aimed at exciting the curiosity of the reader, and these complements are a real added value to the book. Exercises are also included, the solutions of which are given at the end of the book. They constitute a very valuable pedagogical tool. The whole of the book is written in a very clear and rigorous way. The publication of a new, up-to-date, textbook of crystallography and crystal physics will be very welcome at a time when crystallography courses are disappearing in most universities throughout the world, although these disciplines represent basic knowledge compulsory for anyone doing material science, Earth science, biochemistry, solid state physics or chemistry.

André Authier Professor Emeritus, Pierre & Marie Curie University, Paris Former President of the International Union of Crystallography Member of the German Academy of Sciences

Preface Crystallography constantly enjoys a new youth, thanks in particular to the spectacular progress in X-ray sources (synchrotron radiation from dedicated facilities and, very recently, free electron X-ray lasers), which make it possible to investigate an extremely broad range of materials. Its contribution is vital in many scientiﬁc and technological areas. It makes it possible, for example, to understand, and even to predict the properties of materials as diverse as high-Tc superconductors, high performance magnets, or biological materials such as proteins. The pharmaceutical industry invests large funds to set up data banks of structures, determined in the crystallized state, of molecules which could become medicines, in order to correlate their conﬁguration to their healing action. Crystallography also is very important in nanoscience, since some materials, when prepared in the form of nano-objects, take on crystal structures which do not exist in the bulk and which necessarily aﬀect their physical and chemical properties. Geophysicists obtain major information about the Earth mantle by investigating crystallized materials under extreme temperature and pressure conditions. In technology, we must mention structural wonders such as thin ﬁlm based artiﬁcial crystals (multilayers and superlattices) of semiconductors or magnetic materials. These have for several years been present in the giant or tunnel magnetoresistance read heads of the hard drives in all our computers. On the other hand, understanding the relation between the structure and the macroscopic properties of crystals opens the way to the use of physical properties with many applications. Thus piezoelectricity, i.e. the production of an electrical voltage under the eﬀect of stress, is the basis of our quartz watches and plays a central role in cell phones. Electro-optical eﬀects, the change in refractive indices under the eﬀect of an electric ﬁeld, entail a change in light propagation in materials. This book is mostly a translation of Symétrie et propriétés physiques des cristaux, published by EDP Sciences, Orsay, France in 2011. It provides the fundamentals underpinning all these research and application areas. In the ﬁrst part, it describes in a clear and thorough way the periodicity of crystals and their symmetry, both at the microscopic level (space groups) and at the macroscopic level (point groups). It includes a presentation of the crystallography of two-dimensional systems such as surfaces and interfaces.

XII

Symmetry and Physical Properties of Crystals

The second part is dedicated to various physical properties of crystals. They are described in the tensor formalism which is natural for them, emphasizing their link with crystal symmetry. We show in particular how a given property is allowed or forbidden by various crystal symmetries, and how the coeﬃcients of the characteristic tensor are related for the various point groups. We deal not only with basic properties such as elasticity and birefringence, but also with properties which are less often dealt with, such as piezoelectricity, optical activity or the electro-optical eﬀects. Each chapter starts with a short presentation of its contents, and almost all chapters are complemented by exercises through which the notions introduced can be concretely applied, and thus mastered. For these exercises to be a real studying tool, the solutions are explicitly given as a ﬁnal separate Chapter 20. Many of the chapters also include a brief complement, intended to give a glimpse into an area related to that of the chapter and to whet the reader’s scientiﬁc appetite, for example on how and what for crystals are grown, with what probes crystal structures can be determined, etc. This book originates in courses we gave at Paris Diderot University and at Grenoble Institute of Technology, France. It is aimed, with no special prerequisite, at students in crystallography, physics and engineering (especially materials science and electrical engineering) curricula, and at PhD students. It should also be a reference book for researchers and engineers involved, in their daily activity, in the properties of crystals. The authors sincerely thank the ﬁve members of the Advisory Editorial Committee for their very valuable suggestions, the vast majority of which were followed. They are also very grateful to Professor André Authier for writing the Foreword, which actually is a very informative chapter on the history of crystallography. The authors intend to correct the mistakes and typos which will, in spite of their eﬀorts, have remained in this ﬁrst edition. Errata sheets will be provided at https://grenoble-sciences.ujf-grenoble.fr/ouvrage/symmetry-crystals Comments from readers are very welcome. Please write to [email protected] Cécile Malgrange, Christian Ricolleau, Michel Schlenker.

Table of symbols a, b, c

Basis vectors of the unit cell in direct space

a, b, c

Lengths of the basis vectors of the unit cell in direct space

a∗ ,

b∗ ,

c∗

Basis vectors of the reciprocal unit cell

a∗ ,

b∗ ,

c∗

Lengths of the basis vectors of the reciprocal unit cell

v0

Volume of the direct unit cell

v0∗

Volume of the reciprocal unit cell

[uvw] < uvw >

Lattice row parallel to the vector ua + vb + wc Set of lattice rows equivalent to [uvw] through all the symmetry operations of the crystal group

(hkl)

Family of lattice planes with Miller indices h, k and l

(hkil)

Family of lattice planes with Miller indices h, k, i and l for a hexagonal lattice

{hkl}

Set of lattice planes equivalent to (hkl) through the symmetry operations of the crystal group

{hkil}

Set of lattice planes equivalent to (hkil) through the symmetry operations of the crystal group, for a hexagonal lattice

dhkl

Distance between two neighboring (hkl) lattice planes, i.e. the lattice spacing of family (hkl)

e 1 , e2 , e3

Basis vectors of an orthonormal frame

{Mij }

The matrix for which Mij is the coeﬃcient located on the i-th row and the j-th column

{aij } = A

Transition matrix for going over from an orthonormal frame to another one

V

Polar vector

V

Axial vector

[T ]

Tensor

Tij

Components, in a given orthonormal axis system, of a rank-2 tensor [T ]. The associated matrix is noted T .

Tijk

Components, in a given orthonormal axis system, of a rank-3 tensor [T ]

XIV

Symmetry and Physical Properties of Crystals

eij

Components of the tensor of displacement gradients, or distorsion tensor, [e]

T

The set of the crystal lattice translations

Gs

Space group

Gp

Point group

[S], Sij

Strain tensor, and its components

[T ], Tij

Stress tensor, and its components

Sα , Tα

Contracted notation (Voigt’s notation) for the tensors [S] and [T ]. α ranges from 1 to 6, so that the components of these tensors form column vectors with 6 rows.

[s], sijkl

Compliance tensor, and its components

[c], cijkl

Stiﬀness tensor, and its components

Θ

Temperature

S

Entropy

E

Electric ﬁeld

D

Electric induction

P

Polarization

[ε], εij ε0 [η], ηij

Relative permittivity (or dielectric constant) tensor, and its components Permittivity (or dielectric constant) of vacuum Electric impermeability tensor, and its components

δij

Kronecker symbol

δijk

Levi-Civita, or permutation, tensor

[G], Gij

Gyration tensor, and its components

[d], dijk

Piezoelectric tensor, and its components

[r], rijk

Linear electro-optic tensor, or Pockels tensor, and its components

[z], zijkl

Quadratic electro-optic tensor, or Kerr tensor, and its components

[p], pijkl

Elasto-optic tensor and its components

[π], πijkl

Piezo-optic tensor and its components

Contents Chapter 1 – Introduction 1.1. Crystal order ..................................................................... 1.2. Order on a macroscopic scale ................................................ 1.3. Order on a microscopic scale ................................................ 1.4. Basic assumptions of geometrical crystallography ..................... 1.5. Anisotropy of physical properties .......................................... 1.6. Remarks on the scope of this book : topics left out ................... Complement 1C. Crystal growth .................................................... 1C.1. Natural growth of single crystals ................................. 1C.2. Crystal growth for scientiﬁc purposes ........................... 1C.3. Industrial crystal growth ........................................... 1C.4. Growth of single-crystal thin ﬁlms ............................... Further reading .................................................................. References .................................................................................

1 1 3 4 6 6 7 8 8 8 9 10 10 11

Chapter 2 – Symmetry operations 2.1. Isometries ......................................................................... 2.2. Symmetry operations. Symmetry elements .............................. 2.2.1. n-fold rotations and axes ........................................... 2.2.2. n-fold rotoinversions and n-fold rotoinversion axes, denoted as n ¯ -fold axes .............................................. 2.2.3. Translations ............................................................ 2.2.4. Screw axes and glide mirrors ...................................... 2.2.5. Note ...................................................................... 2.3. Introduction to symmetry groups .......................................... 2.4. Exercises ..........................................................................

13 13 14 14

Chapter 3 – Crystal lattices 3.1. Direct lattice ..................................................................... 3.1.1. Unit cell, row .......................................................... 3.1.2. Lattice planes .........................................................

23 23 23 28

15 16 17 18 18 20

XVI

Symmetry and Physical Properties of Crystals

3.1.3. Wigner-Seitz cell ...................................................... Reciprocal lattice ............................................................... 3.2.1. Introduction based on diﬀraction ................................ 3.2.2. Alternative deﬁnition of the reciprocal lattice ................ 3.2.3. Properties of the reciprocal lattice ............................... 3.2.4. Crystallographic calculations ...................................... 3.3. Properties of crystal lattices ................................................. 3.3.1. Centers of symmetry ................................................ 3.3.2. n-fold and n ¯ -fold axes consistent with the crystalline state 3.3.3. The direct lattice and the reciprocal lattice have the same symmetry elements ...................................... 3.3.4. Geometrical relation between the symmetry axes and the crystal lattice ............................................... 3.3.5. The lattice is at least as symmetrical as the crystal ........ 3.4. Crystal systems ................................................................. 3.4.1. Two-dimensional crystal systems ................................. 3.4.2. Three-dimensional crystal systems ............................... 3.5. Examples of reciprocal lattices .............................................. 3.5.1. Monoclinic lattice .................................................... 3.5.2. Orthorhombic, tetragonal and cubic lattices .................. 3.6. Hexagonal lattice and rhombohedral lattice ............................. 3.6.1. Hexagonal lattice ..................................................... 3.6.2. Rhombohedral lattice ............................................... 3.7. Bravais lattices .................................................................. 3.7.1. Why they are needed ................................................ 3.7.2. The fourteen Bravais lattices ...................................... 3.7.3. Reciprocal lattices of the non-primitive lattices .............. 3.8. Surface crystal lattice ......................................................... 3.8.1. Cut surface ............................................................. 3.8.2. Real surface ............................................................ 3.8.3. Notations ............................................................... 3.8.4. Reciprocal lattice ..................................................... 3.9. Exercises .......................................................................... Appendix 3A. The metric tensor ................................................... 3A.1. Deﬁnition ............................................................... 3A.2. Volume of the unit cell .............................................. 3A.3. Product of the matrices associated to the direct and reciprocal metric tensors ...................................... 3A.4. Calculation of lattice distances ................................... 3A.5. Applications ............................................................ 3.2.

32 32 32 34 35 37 40 40 40 41 42 43 43 43 44 47 47 47 48 48 48 50 50 52 53 54 55 55 56 58 59 63 63 63 64 65 65

Contents Chapter 4 – Relationship between space groups and point groups 4.1. Introduction ...................................................................... 4.2. Symmetry operations of the crystal ....................................... 4.2.1. Change in origin ...................................................... 4.2.2. The operations (S, t) form a group .............................. 4.2.3. The lattice translations form an invariant subgroup of the group of symmetry operations of the crystal ......... 4.3. Space groups and point groups ............................................. 4.4. Exercises .......................................................................... Complement 4C. Probes used for crystal structure determination ......... 4C.1. Possible probes and criteria for choice .......................... 4C.2. X-rays .................................................................... 4C.3. Neutrons ................................................................ 4C.4. Electrons ................................................................ Further reading .................................................................. Appendix 4A. General features of groups ........................................

XVII

67 67 70 70 71 72 73 75 76 76 76 78 79 79 80

Chapter 5 – Point groups 83 5.1. Introduction ...................................................................... 83 5.2. Stereographic projection ...................................................... 84 5.2.1. Deﬁnition ............................................................... 84 5.2.2. Examples ............................................................... 86 5.2.3. Application to rotoinversion axes or n ¯ -fold axes ............. 88 5.2.4. Family of equivalent directions ................................... 89 5.3. Improper groups ................................................................ 89 5.3.1. Preliminary remark .................................................. 89 5.3.2. Properties of improper groups .................................... 90 5.4. Enumeration of the proper point groups ................................. 91 5.4.1. Preamble ................................................................ 91 5.4.2. Groups containing only the symmetry operations associated to an axis An (cyclic groups) ....................... 92 5.4.3. Groups containing the symmetry operations associated to an axis An and to a perpendicular axis A2 , or dihedral groups .................................................... 92 5.4.4. Cubic proper groups ................................................. 93 5.5. Enumeration of the improper point groups .............................. 94 5.5.1. Improper groups containing inversion ........................... 94 5.5.2. Improper groups which do not feature inversion ............. 97 5.6. Classiﬁcation of the point groups .......................................... 101

XVIII

Symmetry and Physical Properties of Crystals

5.7. Laue classes ...................................................................... 5.8. Plane point groups ............................................................. 5.9. Isotropy point groups .......................................................... 5.10. Exercises .......................................................................... Appendix 5A. Complements on the stereographic projection ............... 5A.1. Stereographic projection of the transform of a given direction through the symmetry operations associated to various symmetry elements .................................... 5A.2. Stereographic projections of the symmetry elements of a cube ................................................................

106 107 107 109 111

111 112

Chapter 6 – Bravais lattices 6.1. Introduction ...................................................................... 6.2. Plane lattices .................................................................... 6.2.1. Group 1 ................................................................. 6.2.2. Group 3 ................................................................. 6.2.3. Group 4 ................................................................. 6.2.4. Group m ................................................................ 6.2.5. Conclusion .............................................................. 6.3. 3-dimensional lattices .......................................................... 6.3.1. Group 1 ................................................................. 6.3.2. Group 2 ................................................................. 6.3.3. Group 3 ................................................................. 6.3.4. Group 4 ................................................................. 6.3.5. Group 222 .............................................................. 6.3.6. Group 23 ................................................................

117 117 118 118 118 119 119 120 120 120 120 122 124 126 127

Chapter 7 – Space groups 7.1. Introduction ...................................................................... 7.2. Enumeration of the operations (S, t) ...................................... 7.2.1. S is a rotation. Deﬁnition of screw axes ........................ ¯ Deﬁnition of glide mirrors .. 7.2.2. S is a rotoinversion, noted S. 7.2.3. Product of a symmetry operation and a translation ........ 7.3. Enumeration of space groups ................................................ 7.3.1. Symmorphic space groups .......................................... 7.3.2. Non-symmorphic space groups .................................... 7.3.3. International Tables for Crystallography ....................... 7.4. Nomenclature .................................................................... 7.5. Examples: space groups of some structures ............................. 7.5.1. TiO2 -type structure (rutile) .......................................

129 129 130 131 134 136 139 139 142 146 149 151 151

Contents

XIX

7.5.2. Metals with close-packed hexagonal structure ................ 7.5.3. Structure of diamond ................................................ 7.6. Exercises .......................................................................... Complement 7C. Structure determination: outline ............................ Further reading .................................................................. References .................................................................................

152 154 155 158 161 162

Chapter 8 – Chemical bonds and crystal structures 8.1. Introduction ...................................................................... 8.2. Ionic bonds ....................................................................... 8.2.1. Nature and properties ............................................... 8.2.2. Bonding energy ....................................................... 8.2.3. Ionic structures with formula AX ................................ 8.2.4. Other cubic structures .............................................. 8.3. Covalent bonds .................................................................. 8.3.1. Nature of covalent bonds ........................................... 8.3.2. Basic property ......................................................... 8.3.3. Examples ............................................................... 8.3.4. Conclusion .............................................................. 8.4. Van der Waals bonds, or molecular bonds ............................... 8.4.1. Nature and properties ............................................... 8.4.2. Example ................................................................ 8.5. Metallic bonds ................................................................... 8.5.1. Nature and properties ............................................... 8.5.2. Examples ............................................................... 8.6. Remarks and conclusions ..................................................... 8.7. Exercises .......................................................................... Complement 8C. Magnetic structures ............................................. Further reading .................................................................. References .................................................................................

163 163 165 165 168 169 171 173 173 174 174 176 177 177 177 178 178 178 180 181 183 185 186

Chapter 9 – Crystal anisotropy and tensors 9.1. Introduction ...................................................................... 9.2. Anisotropic continuous medium ............................................ 9.3. Representing a physical quantity by a tensor ........................... 9.3.1. Example: electrical conductivity ................................. 9.3.2. A refresher on orthonormal frame changes .................... 9.3.3. Application to electrical conductivity ........................... 9.4. Tensors ............................................................................ 9.4.1. Deﬁnition of a tensor ................................................

187 187 188 189 189 191 193 194 194

XX

Symmetry and Physical Properties of Crystals

9.4.2. An important property ............................................. 9.4.3. Field tensors and material tensors ............................... 9.5. Symmetry properties of tensors ............................................. 9.5.1. Internal symmetry. Symmetric and antisymmetric tensors 9.5.2. External symmetry of material tensors. Curie’s and Neumann’s principles ................................ 9.6. Reduction in the number of independent coeﬃcients of a material tensor ............................................................ 9.6.1. Method using the transformation matrix ...................... 9.6.2. “Direct inspection” method ........................................ 9.6.3. Special case: central symmetry (inversion symmetry) ...... 9.7. Exercises .......................................................................... References ................................................................................. Chapter 10 – Second-rank tensors 10.1. Introduction ...................................................................... 10.1.1. Symmetric and antisymmetric tensors .......................... 10.1.2. Matrix form of second-rank tensors ............................. 10.1.3. Trace ..................................................................... 10.2. Representative quadric for a symmetric rank-2 tensor ............... 10.2.1. Characteristic surface ............................................... 10.2.2. Principal axes and principal coeﬃcients ........................ 10.2.3. Shape of the quadric ................................................. 10.3. Properties of the quadric ..................................................... 10.3.1. Normal to the quadric .............................................. 10.3.2. Length and physical meaning of the radius vector .......... 10.3.3. Intensity of a physical property in a given direction ........ 10.4. Geometrical determination of the principal axes and principal coeﬃcients: the Mohr circle construction ................................ 10.5. Eﬀect of crystal symmetry ................................................... 10.5.1. Triclinic system ....................................................... 10.5.2. Monoclinic system .................................................... 10.5.3. Orthorhombic system ............................................... 10.5.4. Uniaxial systems: rhombohedral, trigonal and hexagonal . 10.5.5. Cubic system .......................................................... 10.6. Axial vectors, or antisymmetric rank-2 tensors ......................... 10.6.1. Polar vectors, axial vectors ........................................ 10.6.2. Example of an axial vector: the cross product ............... 10.7. Exercises ..........................................................................

195 196 197 197 197 200 200 201 202 203 204 205 205 205 206 206 207 207 207 209 210 210 211 211 213 215 216 216 216 217 217 218 218 220 222

Contents

XXI

Chapter 11 – The stress tensor 11.1. Introduction ...................................................................... 11.2. Stress tensor ..................................................................... 11.2.1. Introduction ........................................................... 11.2.2. Deﬁnition of the stress tensor ..................................... 11.2.3. Normal stress and shear stress .................................... 11.3. Basic relation .................................................................... 11.4. Symmetry of the stress tensor ............................................... 11.5. Examples of stress tensors ................................................... 11.5.1. Uniaxial stress ......................................................... 11.5.2. Pure shear .............................................................. 11.5.3. Hydrostatic pressure ................................................. 11.6. Eﬀect of gravity ................................................................. 11.7. Exercises .......................................................................... References .................................................................................

225 225 225 225 227 229 230 233 234 234 235 235 236 238 240

Chapter 12 – Deformation of a solid. The strain tensor 12.1. Distortion tensor (displacement gradient tensor) ...................... 12.1.1. Deﬁnition ............................................................... 12.1.2. Physical meaning of components eij ............................ 12.2. Decomposition of the distortion tensor into a rotation and a strain .................................................. 12.2.1. Introduction using a simple example ............................ 12.2.2. Expressing the distortion associated to small rotations .... 12.2.3. Strain tensor ........................................................... 12.3. Elongation in a given direction ............................................. 12.4. Volume expansion (volumetric strain) .................................... 12.5. Special cases of strain ......................................................... 12.5.1. Simple elongation .................................................... 12.5.2. Pure shear strain ..................................................... 12.5.3. Simple shear strain ................................................... 12.6. Thermal expansion ............................................................. 12.7. Exercises ..........................................................................

241 241 241 243

Chapter 13 – Elasticity 13.1. Introduction ...................................................................... 13.2. Compliance and stiﬀness tensors ........................................... 13.2.1. Generalized Hooke’s law ............................................ 13.2.2. Symmetry of the compliance and stiﬀness tensors ...........

259 259 262 262 263

244 244 245 246 247 248 249 249 249 250 250 254

XXII

Symmetry and Physical Properties of Crystals

13.3. Contracted notation (Voigt’s notation) ................................... 13.3.1. Stress tensor ........................................................... 13.3.2. Strain tensor ........................................................... 13.3.3. Compliance tensor and stiﬀness tensor ......................... 13.3.4. Relation between the compliance and stiﬀness tensors ..... 13.4. Energy of a strained solid .................................................... 13.5. Eﬀect of crystal symmetry on the form of the elastic tensor ........ 13.5.1. Center of symmetry .................................................. 13.5.2. Groups 2, m and 2/m ............................................... 13.5.3. Groups 222, mmm and mm2 ...................................... 13.5.4. Groups 422, 4mm and 4/m mm .................................. 13.5.5. Cubic system .......................................................... 13.6. Isotropic materials .............................................................. 13.6.1. Expressing components sαβ as a function of E and ν ...... 13.6.2. Stiﬀness components. Lamé coeﬃcients ........................ 13.7. Representative surface for Young’s modulus ............................ 13.8. Compressibility .................................................................. 13.8.1. Bulk compressibility ................................................. 13.8.2. Linear compressibility of a bar .................................... 13.9. Notes on non-uniform stresses and strains ............................... 13.10. Exercises .......................................................................... Complement 13C. Plastic deformation and crystal defects .................. Further reading .................................................................. References .................................................................................

264 264 265 265 268 268 271 274 274 274 275 276 276 278 279 279 281 281 282 283 285 288 290 291

Chapter 14 – Elastic waves in crystals 14.1. Introduction ...................................................................... 14.2. Plane elastic waves ............................................................. 14.3. Application to a cubic crystal ............................................... 14.3.1. Propagation of a plane wave along direction [100] ........... 14.3.2. Propagation along direction [110] ................................ 14.4. Isotropic solid case ............................................................. 14.5. Microscopic approach – Crystal lattice dynamics ...................... 14.5.1. Linear chain of identical atoms ................................... 14.5.2. Linear chain with two diﬀerent atoms .......................... 14.5.3. Extension to the real crystal case ................................ 14.6. Exercises ..........................................................................

293 293 294 297 298 299 300 301 301 305 308 309

Contents

XXIII

Chapter 15 – Crystal thermodynamics. Piezoelectricity 15.1. Crystal thermodynamics ...................................................... 15.1.1. Conjugate variables .................................................. 15.1.2. Independent variables ............................................... 15.1.3. Principal eﬀects vs crossed eﬀects ............................... 15.1.4. Summary of the various eﬀects ................................... 15.1.5. Condensed representation of the physical property matrix 15.2. Pyroelectricity. Pyroelectric crystals ...................................... 15.3. Piezoelectric crystals ........................................................... 15.3.1. Direct eﬀect and inverse eﬀect .................................... 15.3.2. Piezoelectric tensor [d] and its two-subscript notation ..... 15.3.3. Eﬀect of crystal symmetry on the form of the tensor ....... 15.3.4. Longitudinal piezoelectricity surface ............................ 15.3.5. Other forms of piezoelectric coeﬃcients ........................ 15.3.6. Applications ........................................................... 15.4. Principal and crossed eﬀects under various conditions ............... 15.5. Exercises .......................................................................... Complement 15C. Electrostriction and magnetostriction .................... Further reading .................................................................. References .................................................................................

311 312 312 314 317 318 320 321 322 322 323 324 328 329 331 332 334 337 338 339

Chapter 16 – Light propagation in crystals 16.1. Maxwell’s equations ............................................................ 16.2. Light propagation in an isotropic material .............................. 16.3. Sinusoidal waves that are solutions of Maxwell’s equations ......... 16.4. Plane monochromatic wave in an anisotropic material ............... 16.4.1. Basic equation ......................................................... 16.4.2. Birefringence ........................................................... 16.4.3. Index surface .......................................................... 16.4.4. Index ellipsoid ......................................................... 16.4.5. Determining the induction vectors ............................... 16.4.6. Direction of energy propagation .................................. 16.5. Refraction of a plane wave at the boundary between two materials 16.5.1. The wave-vectors follow the Snell-Descartes law ............. 16.5.2. Application to uniaxial materials ................................ 16.6. Conclusion ........................................................................ 16.7. Exercises ..........................................................................

341 341 342 343 345 345 346 347 349 350 353 354 354 357 358 360

XXIV

Symmetry and Physical Properties of Crystals

Appendix 16A. Wave surface (or ray surface) and Huygens’ construction 364 16A.1. Wave surface (or ray surface) .................................... 364 16A.2. Huygens’ construction ............................................. 367 Chapter 17 – Polarization of light by crystals 17.1. Polarization state of an electromagnetic wave .......................... 17.1.1. Linearly polarized wave ............................................. 17.1.2. Circularly polarized wave .......................................... 17.1.3. Elliptically polarized wave ......................................... 17.1.4. Natural light ........................................................... 17.2. Jones notation ................................................................... 17.3. Linear polarizers ................................................................ 17.4. Phase-shifting plates ........................................................... 17.4.1. Half-wave plates ...................................................... 17.4.2. Quarter-wave plates ................................................. 17.5. Partially polarized waves and Stokes parameters ...................... 17.6. Exercises .......................................................................... References .................................................................................

369 369 370 370 372 372 373 374 376 377 378 379 382 384

Chapter 18 – Rotatory power and optical activity 18.1. Deﬁnition of the rotatory power of a material .......................... 18.2. Fresnel’s interpretation ........................................................ 18.3. Interpretation of rotatory power through the inﬂuence of the local environment ...................................................... 18.3.1. Eﬀect of spatial dispersion ......................................... 18.3.2. Wave propagation in optically active crystals ................ 18.4. Eﬀect of crystal symmetry on the gyrotropy tensor ................... 18.4.1. Centrosymmetric groups ............................................ 18.4.2. Non-centrosymmetric groups ...................................... 18.5. Rotatory power and chirality ................................................ 18.6. Absorption and conclusion ................................................... Complement 18C. Magnetic optical rotation .................................... Further reading .................................................................. Appendix 18A. Axial tensors, or pseudo-tensors ............................... 18A.1. Deﬁnition of axial tensors, or pseudo-tensors ................. 18A.2. Levi-Civita tensor, or permutation tensor ...................... 18A.3. The gyrotropy tensor [G] is a rank-2 axial tensor ............ 18A.4. Relation between tensors [G] and [β] ............................ References .................................................................................

385 385 386 388 388 390 393 393 394 396 400 401 402 403 403 403 404 405 406

Contents

XXV

Chapter 19 – Electro-optical and elasto-optical eﬀects 19.1. Introduction ...................................................................... 19.2. Electro-optical eﬀects .......................................................... 19.2.1. Linear electro-optical eﬀect, or Pockels eﬀect ................. 19.2.2. Applications of the linear electro-optical eﬀect ............... 19.2.3. Quadratic electro-optical eﬀect, or Kerr eﬀect ................ 19.3. Elasto-optical eﬀects ........................................................... 19.3.1. Deﬁnition ............................................................... 19.3.2. Application to the acousto-optical eﬀects ...................... 19.4. Exercises .......................................................................... Complement 19C. Frequency doubling, or Second Harmonic Generation Further reading ..................................................................

407 407 408 408 415 420 424 424 427 430 433 434

Chapter 20 – Solutions to the exercises 20.1. Exercises for Chapter 2 ....................................................... 20.2. Exercises for Chapter 3 ....................................................... 20.3. Exercises for Chapter 4 ....................................................... 20.4. Exercises for Chapter 5 ....................................................... 20.5. Exercises for Chapter 7 ....................................................... 20.6. Exercises for Chapter 8 ....................................................... 20.7. Exercises for Chapter 9 ....................................................... 20.8. Exercises for Chapter 10 ...................................................... 20.9. Exercises for Chapter 11 ...................................................... 20.10. Exercises for Chapter 12 ...................................................... 20.11. Exercises for Chapter 13 ...................................................... 20.12. Exercises for Chapter 14 ...................................................... 20.13. Exercises for Chapter 15 ...................................................... 20.14. Exercises for Chapter 16 ...................................................... 20.15. Exercises for Chapter 17 ...................................................... 20.16. Exercises for Chapter 19 ......................................................

435 435 436 444 445 450 456 458 459 461 463 470 475 479 487 492 499

General references

507

Index

511

Chapter 1

Introduction This chapter introduces the spatial periodicity and the macroscopic scale symmetry properties which characterize crystals.

1.1. Crystal order Depending on temperature and pressure, all materials take on three diﬀerent states: solid (S), liquid (L) and gas (G) (Fig. 1.1). However, when looking at matter from a microscopic point of view, there are only two really distinct states: the ordered state (grey area on Fig. 1.1) and the disordered state. It is clear that a gas at low pressure, consisting of a set of molecules separated by distances that are large compared to their size, is totally disordered. In a liquid, the molecules are in contact with one another, like marbles packed in a bag. A liquid is not completely disordered: there is some order, but only at short range. Furthermore, it is possible to go continuously from the gas state to the liquid state. At a temperature Θ between the temperature ΘT of the triple point and that ΘC of the critical point, a gas undergoing compression goes from the gas state (A) to the liquid state (B) through a sharp transition, liquefaction or condensation. But it is possible to go from A to B around the critical point, for instance by going from A to D at constant pressure, then from D to F at constant temperature, and then from F to B at constant pressure. In contrast, it is impossible to go from the disordered area to the ordered area without crossing the line, shown as a thick line on the ﬁgure, that clearly separates the ordered and the disordered domains. This line consists of two parts: one corresponds to sublimation (solid–gas transition) and to condensation for the inverse transformation, the other to melting (solid–liquid transition) and to solidiﬁcation for the inverse transformation. The equilibrium diagram of Figure 1.1 applies to most solids and their transition to a disordered state, either liquid or gas. However, for some solids, the liquid–solid transition is not sharp but continuous: this is the case for amorphous or glassy solids. When the temperature of such a material in liquid form is lowered, its viscosity increases, which means that its ﬂow is more and

© Springer Science+Business Media Dordrecht 2014 C. Malgrange et al., Symmetry and Physical Properties of Crystals, DOI 10.1007/978-94-017-8993-6_1

1

2

Symmetry and Physical Properties of Crystals p

melting curve ordered state

disordered state

S

B

F C

G L T

A

D

sublimation curve T

C

T

Figure 1.1: Equilibrium diagram for a pure substance, in a representation where pressure p is shown as a function of temperature T more diﬃcult. It forms a kind of paste, which ends up being solid but with a structure hardly more ordered than that of a liquid: it is a kind of set liquid – which corresponds to a metastable state. This book deals only with crystalline solids, characterized by long-range order. The size of the ordered regions depends on the conditions in which crystallization occurs. If no special care is exercised when solidifying a pure liquid, microcrystals appear at various points of the liquid, grow and end up being contiguous. Each small crystal is perfectly ordered, but there is no reason for these crystals to have the same orientation. We get a polycrystal, i.e. a solid made up of small crystals (grains) with the same structure, but diﬀerently oriented. This is the most prevalent case for materials and in particular for metals (Fig. 1.2). However, some minerals occur in single crystal form, i.e. in a form where the solid is identically oriented over its entire volume. This is the case for the gems of jewelers, and for some beautiful minerals which can be found in private or public collections1 (Fig. 1.3a). On the other hand, some crystals can be manufactured in the form of quite large single crystals. This is the case for silicon or quartz, which are produced as single crystals several tens of centimeters in size (Fig. 1.3b).

1. All museums of natural history have a section on minerals. If you visit Paris (France), you will enjoy in particular the mineral collection of Pierre & Marie Curie University (UPMC) and of the Institut de Minéralogie et de Physique des Milieux Condensés (IMPMC), located at 4 place Jussieu, in the 5th district (arrondissement).

Chapter 1 – Introduction

3

Figure 1.2: Scanning Electron Microscopy (SEM) image of the surface of a polycrystalline copper sample (courtesy Cyril Langlois)

(a)

5 cm

(b)

5 cm

Figure 1.3: (a) A sample of pyrite (iron sulﬁde, FeS2 ), mineral collection of Pierre & Marie Curie University (Paris 6) (photograph by Jean-Pierre Boisseau); (b) two bars of single crystal synthetic quartz produced by the SICN company (photograph by Alain Jeanne-Michaud)

1.2. Order on a macroscopic scale The existence of crystal order was sensed in the 17th century at the macroscopic scale, and recognized at the beginning of the 20th century at the microscopic scale. For instance, Niels Stensen, or Nicolaus Stenonius, or Steno, a Dane, noticed as early as 1669 that the angles between faces of natural crystals of quartz and some other minerals have a well deﬁned, constant value, independent of their origin. He then spelled out the law of constancy of angles, which was to be generalized to all crystals by Romé de l’Isle in 1783. This constancy of angles also shows up on the small crystals which form naturally during solidiﬁcation. The mineralogist René Just Haüy showed in 1784 how this regularity in angles can be explained. He had noticed that, when he would cleave2 a crystal of calcite, he would obtain smaller and smaller rhombohedra, all with the same 2. When a crystal of calcite is broken, the fracture surface features perfectly plane areas, with a restricted number of orientations. If one attempts, using a cutting tool and a small hammer, to cleave the crystal, i.e. to break it along one of these special areas, one obtains, provided the blade is properly oriented and the experimentalist has some experience, two fragments separated by a beautiful plane suface known as a cleavage surface.

4

Symmetry and Physical Properties of Crystals

angles. He then imagined that a ﬁnal stage, i.e. a small elementary rhombohedron which can no more be cut, should eventually be reached. He deduced that the macroscopic crystal should be formed from the regular stacking of small rhombohedra, all identical to this elementary rhombohedron which he called the “integrating molecule”. He then showed, and this is the strong point of his theory, that he could reconstruct all external forms of crystals by stacking identical elementary parallepiped-shaped blocks into successive layers which he shifted by a constant, integral number of units at each layer (Fig. 1.4). The parameters deﬁning the basic parallelepiped were characteristic of the crystal. The notions of periodicity and of crystal unit cell, which we will deﬁne later, thus appear.

Figure 1.4: A stacking of layers of identical parallelepipeds, regularly shifted to reproduce the actual habit of the crystal

1.3. Order on a microscopic scale After Haüy and until 1912 the concepts of symmetry and of internal periodicity in the crystal developed. However it was not evident, or at any rate not proved, that this internal order, viz. a triply periodic stacking, could exist in materials with any external shape. It was in fact through the discovery of X-ray diﬀraction by Max von Laue in 1912, and thanks to the work of William and Lawrence Bragg, that the existence of a periodic stacking of atoms in solids, as predicted by Haüy, could be evidenced. They showed that X-rays are diﬀracted by crystals along special directions, forming a discrete set of spots which could be interpreted only

Chapter 1 – Introduction

5

through a triply periodic stacking of the atoms. Thus crystalline solids can be represented using a crystal motif,3 comprising a ﬁnite number of atoms, periodically repeated along three non-coplanar directions with periods along these directions respectively a, b and c. Let us discuss a few examples to illustrate this notion of periodicity. Figure 1.5 shows a frieze formed by repeating, with period a, a motif. Figure 1.6 shows a sample of wallpaper featuring periodicity in two directions (periods a and b).

a

Figure 1.5: A decorative pattern from Arabic art, after J. Bourgoin, Arabic Geometrical Pattern and Design (Dover Publications, New York, 1973)

b a

Figure 1.6: A sample of wallpaper A crystal is thus formed from a motif consisting of a set of atoms. Repeating the motif through a translation a leads to a kind of linear crystal. If this linear crystal is submitted to a translation by a vector b (not collinear with a), then by 2b, 3b, etc., a plane crystal is obtained. To obtain the global crystal, the plane crystal is then thought to be submitted to a translation by a vector c not coplanar with plane (a, b), then by 2c, 3c, etc. 3. Motif is the French word for pattern. It is adopted in crystallographic English, with the present meaning.

6

Symmetry and Physical Properties of Crystals

1.4. Basic assumptions of geometrical crystallography In order to describe crystal structures, we make three assumptions: 1.

The crystal is assumed to be inﬁnite. This assumption is reasonable, since the order of magnitude of the lengths a, b and c of the period vectors is a few angströms (1 Å = 10−1 nm). A small crystal with dimensions of the order of a micrometer, for example, contains linear sequences several thousands of periods long.

2.

The thermal vibrations of atoms about a perfectly deﬁned average position is neglected. Our description assumes that the atoms are ﬁxed at these average positions.

3.

The crystal is assumed to be perfectly triply periodic, i.e. not to feature any defect. Crystal defects can then be described with respect to the perfect crystal. The study of crystal defects is a broad subject, outside the scope of this book. A brief introduction to one type of defect, the dislocation line, is given in Complement 13C.

1.5. Anisotropy of physical properties The beautiful crystal faces that can be observed in natural minerals and in some synthetic crystals are related to the very strong anisotropy of the growth rates as a function of growth direction. Figure 1.7 explains how the only faces that remain after some growth has occurred are those perpendicular to the directions where the growth rate is much smaller than in other directions. We consider, at time t = 0, three face orientations denoted as 1, 2 and 3, with one of them (noted 2) growing at a velocity v2 twice larger than the two others (faces 1 and 3). We see that at time t all faces are present, whereas, at time 2t, face 2 has disappeared.

v2t

v1t 1

2 v1t

2 3

t=0

t

2t

Figure 1.7: Growth at diﬀerent rates of crystal faces. Face 2, with growth velocity v 2 twice larger than that, v 1 , of faces 1 and 3, ends up disappearing.

Chapter 1 – Introduction

7

The habit, i.e. the very regular special shape, of crystals thus shows that the growth velocity is much smaller along certain directions, ﬁnite in number, than in all other directions. This is one of the expressions of the anisotropy of the physical properties of crystals. In this case, anisotropy is discontinuous while, for most other physical properties, it is continuous, meaning that the value of a physical quantity such as the expansion of a material along a given direction, under the inﬂuence of a rise in temperature, varies continuously as direction is varied. This anisotropy of their physical properties is a characteristic of crystals. Describing it involves the use of tensors. This will be the topic of the second part of this book, starting with Chapter 9.

1.6. Remarks on the scope of this book : topics left out The aim of this book is to describe the structure and properties of perfectly ordered crystalline solids. We have seen that we therefore leave aside glasses or amorphous solids, the structure of which is close to that of a liquid set at a given instant [1]. Neither shall we mention liquid crystals or mesophases [2]. They often consist of rod-shaped molecules, which assemble parallel to one another, forming plane layers. In a given layer, the molecules may be ordered only at short range, as in a liquid, but the existence of these parallel layers denotes partial order, whence the term crystal. Neither will we deal with quasi-crystals, discovered in 1984 [3] (see also [4]). They can be obtained through ultra-fast quenching of metallic alloys (e.g. Al–Mn–Si or Al–Fe–Cu). They do not feature the triple periodicity of crystals. They do however, like crystals, feature orientation symmetry: all properties observed along a given direction are reproduced along the directions deduced from the former through the action of the symmetry elements in the point group of the quasi-crystal. Because there is no translation symmetry, these point groups are diﬀerent from those that are consistent with the crystalline state.

8

Symmetry and Physical Properties of Crystals

Complement 1C. Crystal growth This complement is no more than a glimpse into the fascinating art and science of crystal growth. The variety of techniques and of characterization methods it encompasses is exempliﬁed by a recent handbook of crystal growth (see Further reading): it comprises over 1800 pages, with a short table of contents spanning 14 pages and a detailed table of contents of 30 pages.

1C.1. Natural growth of single crystals The largest producer of single crystals is nature. Large (centimeter-range) single crystals of many naturally occurring compounds, usually called minerals, have long been valued for their beauty and have raised many questions that led to understanding the structure of matter. Their characteristic habits, with well-developed natural faces, occur when their growth process involves isotropic enough an environment as well as enough space. The typical process, hydrothermal growth, is based on the slow deposition of a solute as the temperature of the solution changes, and it is often associated with high pressures. Among the most popular examples of minerals are quartz SiO2 (rock crystal), calcite CaCO3 (Iceland spar), diamond C, pyrite FeS2 (fool’s gold, Fig. 1.3a). They may well, through their beauty, have kindled the reader’s interest for crystals and symmetry. Other materials crystallize very easily, at room pressure and room temperature, from solutions: this is the case for sodium chloride NaCl (rocksalt), or copper sulfate CuSO4 . Crystallization is then a convenient way of purifying the material.

1C.2. Crystal growth for scientiﬁc purposes Growing single crystals is an important support activity for basic research. A meaningful investigation of anisotropic macroscopic properties, for example magnetism, electrical or heat conduction, or the ferroelectricity (see Sect. 15.2) of materials, requires single crystals, where the directional properties are the same throughout the sample. The growth must then be followed by the precise determination of the orientation of the crystal, so that a sample with well-deﬁned crystal directions can be cut out. The laboratory techniques cover a broad range of approaches, depending on the chemical properties, melting temperature, etc. of the material. Thus soluble materials can often be made to crystallize in a controlled way by slow evaporation of the solvent, while refractory materials will have to be molten in an induction furnace, often in the form of a levitating drop without contact with a crucible to avoid contamination, and cooled in a temperature gradient. The Bridgman method provides for cooling of a larger molten sample, in contact with a small crystal used as a seed, in a temperature gradient. Another broadly used technique is the Czochralski method, where the seed is dipped into the melt and slowly pulled out at the same time that it is rotated. In the ﬂux-growth method, the material to be crystallized is molten together with another material which is

Chapter 1 – Introduction

9

not incorporated in the solid but lowers the melting temperature; with proper setting of the temperature evolution over days or weeks, good crystals can be obtained. From another point of view, single crystals are necessary for many structure determinations using X-ray or neutron diﬀraction techniques. However, detailed examination of the validity of the usual data processing procedures (“kinematical approximation”, if necessary with corrections) indicates that the crystals should not be big. Typical optimal sizes are tenths of a millimeter for X-rays, and a few millimeters for neutrons. Furthermore, nearly perfect crystals are not desirable for this kind of study, so that the requirements are, happily, close to what crystal synthesis produces. The preparation of single crystals of biological material, such as proteins, in their native hydrated form, is a crucial step toward the determination of their structure. The approach usually consists in trying many recipes at the same time, using boxes with tens of compartments which are ﬁlled with drops of the material with various values of the pH or other possibly relevant parameters. The growth of crystals of biomaterials was investigated in microgravity conditions in satellites, in order to eliminate the inﬂuence of convection. A similar quest is the motivation for crystal growth in gels.

1C.3. Industrial crystal growth It may appear paradoxical to ﬁnd that almost perfect crystals, the production of which is almost invariably fraught with diﬃculties, are required by industry rather than by basic research. Semiconductor device production is based on the preparation of many chips per single-crystal silicon substrate. They are cut from huge single crystal ingots, typically 300 mm in diameter in 2009 and a meter long, without any linear defect (dislocation line, see Complement 13C). This achievement in crystal growth technology was the result of large eﬀorts toward a thorough understanding of crystal defects. These eﬀorts were undertaken because it was vital to keep at a very low level the number of defective chips grown on a wafer. One side-eﬀect of the mastery achieved in the preparation and processing of silicon crystals was that elaborately shaped parts like inkjet printer nozzles were made out of silicon single crystals. Crystals with intermediate sizes are grown industrially for applications in optoelectronics (for example lithium niobate LiNbO3 – see Sect. 19.2). Other materials routinely produced in the form of excellent crystals, but comparable neither in quantities nor in quality with silicon, are SiO2 (quartz) and AlPO4 (berlinite) for piezoelectric oscillators (see Chap. 15), and SiC (silicon carbide) for electronic devices. Industrial single crystals of diamond are available in a wide range of crystal quality and crystal size, with use as diﬀerent as oil drill rigs and optical elements (monochromators) for synchrotron radiation X-rays. Synthetic diamond does not reach into the jewelry range yet, but other gemstones (emerald, sapphire. . . ) are routinely produced artiﬁcially as substitutes for their natural

10

Symmetry and Physical Properties of Crystals

counterparts. Again in a very diﬀerent area, turbine blades for jet planes are made of single crystals of an aluminum-base alloy in view of their mechanical strength at the high temperatures involved.

1C.4. Growth of single-crystal thin ﬁlms Films with very small thickness, down to the nanometre range, are important for nanotechnology and basic science, e.g. for the investigation of semiconductor quantum well or quantum dot devices, or of magnetic recording and readout heads for hard disk drives. Their manufacture involves a range of approaches, based on vapor-phase or liquid-phase epitaxy (the growth of single crystal ﬁlms on single-crystal substrates, with a close relation between their orientations), or molecular-beam epitaxy (MBE). The latter is a highly sophisticated technique involving extreme vacuum and requiring stringent purity controls. Multilayers, consisting of several stacked thin ﬁlms exhibiting structural coherence at the interfaces, are industrially manufactured by sputtering techniques. They make up the tunnel magnetoresistance (TMR) read heads4 used in 2011 in the hard disk drive of all recent computers. Mastering epitaxic growth processes implies a very good knowledge of the surfaces on which the layers are to be grown. This makes the study of surface crystallography very important. The description of crystal surfaces is dealt with in Section 3.8 of this book.

Further reading I.V. Markov, Crystal Growth for Beginners (World Scientiﬁc, Singapore, 1996) G. Dhanaraj, K. Byrappa, V. Prasad, M. Dudley, Springer Handbook of Crystal Growth (Springer, 2010)

4. Wikipedia, Tunnel magnetoresistance, http://en.wikipedia.org/wiki/Tunnel magnetoresistance (as of Nov. 7, 2013)

Chapter 1 – Introduction

11

References [1] S.R. Elliot, Physics of Amorphous Materials, 2nd edn. (Longman Scientiﬁc and Technical, Harlow, Essex, 1990) [2] P.G. de Gennes and J. Prost, The Physics of Liquid Crystals (Oxford University Press, Oxford, 1993) [3] D. Shechtman, I. Blech, D. Gratias, J.W. Cahn, Metallic phase with longrange orientational order and no translational symmetry, Phys. Rev. Lett. 53, 1951–1953 (1984) [4] C. Janot and J.M. Dubois, Les quasicristaux, matière à paradoxes (EDP Sciences, Les Ulis, 1998)

Chapter 2

Symmetry operations The aim of this chapter is to detail the notions of symmetry operations and symmetry elements, which are basic in the description of crystals. The ﬁnal section introduces some notions related to symmetry groups.

2.1. Isometries An isometry is a geometrical transformation which transforms an object either into an identical object (this is called a direct or proper isometry) or into its image with respect to a mirror plane (it is then called an indirect or improper isometry). A direct, or orientation preserving, isometry conserves the handedness (right or left) of a trihedron, whereas an indirect, or orientation reversing, isometry reverses it. Successively applying two isometries, i.e. applying the composition or “product” of these isometries obviously is an isometry. The product of two direct isometries is a direct isometry since the transform is at each stage identical to the object. The product of a direct and an indirect isometry is an indirect isometry, and the product of two indirect isometries is a direct one. More generally, the product of any number of isometries is indirect if it involves an odd number of indirect isometries, and a direct isometry otherwise. The isometries are: a rotation around a given axis, a translation (both of these are direct isometries), symmetry with respect to a point, also called inversion with respect to this point, symmetry with respect to a plane (both being indirect isometries), and all operations resulting from the composition (or product) of two or several of these isometries. It is convenient to deﬁne a special indirect isometry which is very much used in crystallography: rotoinversion (or rotation-inversion), the product of a rotation around an axis and of an inversion with respect to a point located on this axis. Two special rotoinversions should be mentioned here: rotoinversion by 2π, which is nothing else than inversion, and rotoinversion with angle π, which is

© Springer Science+Business Media Dordrecht 2014 C. Malgrange et al., Symmetry and Physical Properties of Crystals, DOI 10.1007/978-94-017-8993-6_2

13

14

Symmetry and Physical Properties of Crystals

equivalent to symmetry with respect to the plane perpendicular to the axis used for the rotation, and going through the point O used for the inversion (Fig. 2.1). z’ m

M

O

H

P M’ z

Figure 2.1: Rotoinversion by π around axis zz , the point used as a center of symmetry being O. M is the transform of M through this rotoinversion because m is the transform of M through a rotation by π around axis zz and M is the transform of m through the symmetry with center O. M is symmetric of M with respect to plane P, perpendicular to zz and going through O. We thus see that the set of isometries can also be deﬁned as the set of the rotations, rotoinversions, translations and their combinations, since inversion and symmetry with respect to a plane are two special rotoinversions.

2.2. Symmetry operations. Symmetry elements For some objects, an isometry (or several isometries) transform(s) the object into an object that is not only identical but superimposable on the object itself, and which is therefore undistinguishable from the latter. These isometries which leave the object invariant are the symmetry operations for this object.

2.2.1. n-fold rotations and axes Consider as an example the two-handled jug shown on Figure 2.2a. A rotation by 180◦ around axis zz changes the jug into a jug that superimposes upon itself: the rotation by 180◦ around zz is a symmetry operation for this object. The product of this symmetry operation with itself is a rotation by 360◦ around zz , or the identity operation since, following this symmetry operation, the object is superimposed upon itself point for point. Axis zz is said to be a 2-fold axis for the jug, or alternatively the jug is said to have a 2-fold axis as a symmetry element. The regular square-based pyramid shown on Figure 2.2b has a 4-fold axis because the rotation by 2π/4 = π/2 around zz is a symmetry operation for this pyramid. The existence of a 4-fold axis implies that the object has 4 symmetry

Chapter 2 – Symmetry operations

15

operations, viz. the rotation by π/2 around the axis, which can for example be noted as R, its product with itself R2 , which is the rotation by π, the product of R2 by R, i.e. R3 , which is the rotation by 3π/2, and operation R4 , equal to the rotation by 2π or identity operation, noted E. In a general way, if an object has an n-fold rotation axis, it has n symmetry elements which are the rotations by 2π/n, 2(2π/n), . . . , k(2π/n) . . . and ﬁnally the rotation by n(2π/n) = 2π which is the identity operation. The cylinder of revolution shown on Figure 2.2c has an inﬁnite-order axis, because a rotation by any angle, however small, is a symmetry operation. z

z

z

z’

z’

z’

(a)

(b)

(c)

P

Figure 2.2: Objects featuring symmetry elements We will see (Sect. 3.3.2) that crystals, because of their triple periodicity, can only have 2-, 3-, 4- or 6-fold axes.

2.2.2. n-fold rotoinversions and n-fold rotoinversion axes, denoted as n ¯ -fold axes If a rotoinversion by angle 2π/n (the product of a rotation by 2π/n around a given axis and an inversion with center O located on this axis) is a symmetry operation for an object, the latter is said to have an n ¯ -fold rotoinversion axis. We have seen that the rotoinversion by 2π is identical with inversion. The existence of a ¯1 axis is therefore equivalent to the existence of a center of symmetry. The existence of a ¯2-fold axis (for which the associated symmetry operation is the rotoinversion by π) is equivalent to the existence of a symmetry plane (or mirror) perpendicular to the axis and going through the center used for inversion (see Fig. 2.1). It should be noted, in contrast, that the axis deﬁning the rotation is not a 2-fold axis for the object, just as the inversion center that is used in this rotoinversion is not a center of symmetry for the object. A rotoinversion is the product of a rotation and an inversion. It is therefore quite distinct from the rotation itself and the inversion itself.

16

Symmetry and Physical Properties of Crystals

We will see that crystals can only have as rotoinversion axes ¯1, ¯2, ¯3, ¯4 or ¯6 axes. An example of an object having a ¯4-axis is shown on Figure 2.3a. It is a sphenohedron, a solid having four vertices A, B, C and D with the following properties: segments AB and CD have equal lengths and are perpendicular to each other. They are perpendicular to the axis zz which intersects them in their middles, H and K respectively (Fig. 2.3b and 2.3c). The rotoinversion by π/2 around zz , with point O, the middle of HK, as the inversion center, transforms point A into C, point B into D, C into B and D into A. It thus transforms the sphenohedron into itself. Axis zz is therefore a ¯4 axis for this solid. In contrast, it is quite clear that the sphenohedron has neither a 4-fold axis nor an inversion center. z’ A B

A

H B

D A O

O, H, K B C D

C

D

K

C z

(a)

(b)

(c)

Figure 2.3: (a) A perspective view of a sphenohedron. (b) The sphenohedron ABCD. Axis zz is a ¯4-fold axis for this object. (c) Projection of points A, B, C and D on a plane perpendicular to zz .

2.2.3. Translations If a translation by a vector t is a symmetry operation for an object, the product of n translations t, equal to the translation nt, is also a symmetry operation. Since n can be arbitrarily large, the object is necessarily inﬁnite, in contrast to the above cases of rotations and rotoinversions. Such an object is said to be periodic with period t. For example, Figures 2.4a and 2.4b, obtained from a simple pattern which is outlined by a thin dotted line (something like a music note for 2.4a and a set of two such notes for 2.4b), repeated to inﬁnity by translation t, have translation t (and all the translations nt) as symmetry operations. Figure 2.4b furthermore has a symmetry plane or mirror, perpendicular to the plane of the ﬁgure and going through the line uu . If the inﬁnite sequence of patterns of Figure 2.4a is submitted to a translation by a vector t (not collinear with t) and its multiples, the obtained ﬁgure (Fig. 2.5) has the translations nt + n t (n and n integers) as symmetry operations.

Chapter 2 – Symmetry operations

17

t

(a)

u

t

u’

(b)

v

t

v’

(c)

Figure 2.4: Figures which are periodic with period vector t (assuming they extend to inﬁnity). The motif or pattern is marked with a thin dotted line on each ﬁgure.

t’ t

Figure 2.5: A plane ﬁgure with periodicity along two directions

2.2.4. Screw axes and glide mirrors In Sections 2.2.1 and 2.2.2, we deﬁned two types of symmetry elements : axes of order n and axes of order n ¯ . In crystallography, further symmetry elements must be deﬁned. They are associated to the symmetry operations which are the products (also called compositions) of rotations or rotoinversions and translations. These elements are on the one hand screw axes, the associated symmetry operations of which are the products of a rotation and a translation parallel to the rotation axis and, on the other hand, glide mirrors, the associated symmetry operations of which are the products of an operation of symmetry with respect to a plane (a mirror operation) and a translation parallel to this plane. Consider two examples: an object with a screw axis and an object with a glide

18

Symmetry and Physical Properties of Crystals

mirror. Since the associated symmetry operations include a translation part, these objects are necessarily inﬁnite. Screw axis: consider a helical staircase, in which all steps have the same height, and such that when walking up by one step we rotate around the central axis by an angle equal to a submultiple of 2π, for example 30◦ . The operation product of a rotation by 30◦ around the axis of the staircase and a vertical translation equal to the height of the steps is a symmetry operation for this staircase, under the proviso, of course, that we imagine it to have inﬁnite height. This staircase has a screw axis coinciding with its axis. Glide mirror: Figure 2.4c is formed from a motif (the pattern of Fig. 2.4b altered by translating one of the two notes by t/2), repeated to inﬁnity by translation t. This periodic ﬁgure thus features translation t and its multiples as symmetry operations. It also features a less obvious symmetry operation: the product of the symmetry with respect to a plane perpendicular to the plane of the ﬁgure and going through line vv and the translation by vector t/2. The corresponding symmetry element is called a glide mirror, the glide being the translation t/2.

2.2.5. Note We have deﬁned the following symmetry elements: n-fold axes, for which the associated symmetry operations are a rotation by 2π/n and its multiples, n ¯ -fold axes, for which the associated symmetry operations are a rotoinversion by 2π/n and its multiples, mirrors for which the associated symmetry operation is symmetry with respect to the plane of the mirror, screw axes for which the associated symmetry operations are the product of a rotation and a translation and its multiples, and glide mirrors, for which the associated symmetry operations are the product of a symmetry with respect to the plane of the mirror and a translation and its multiples. We see that the term “symmetry element” covers two notions: on the one hand a geometrical object, a line or a plane, and on the other hand the set of symmetry operations which are associated to it.

2.3. Introduction to symmetry groups In this introduction, we restrict discussion to ﬁnite objects. This rules out symmetry operations that include a translation. The symmetry operations which a ﬁnite object can feature are thus the rotations and rotoinversions, the latter including symmetry with respect to a point and symmetry with respect to a plane (Sect. 2.1 and Fig. 2.1). We show that the symmetry operations of a ﬁnite object form a group. Let us ﬁrst recall the deﬁnition of a group.

Chapter 2 – Symmetry operations

19

A group is a set of elements among which one can deﬁne an internal composition law that is associative and includes a neutral element e such that, for any element a of the group, ae = ea = a. Each element of the group must have an inverse a−1 such that aa−1 = a−1 a = e. For the symmetry operations featured by an object, the internal composition law is the product of two symmetry operations, i.e. the succession of these two operations. The neutral element is the identity operation, and the inverse operations of the elementary operations, such as rotation by an angle ϕ around an axis, symmetry with respect to a point O or symmetry with respect to a plane P are thus evident: they are respectively the rotation by an angle −ϕ around the same axis, symmetry with respect to the same point O, and symmetry with respect to the same plane P. The symmetry operations of an object thus form a group. Let us take as an example the symmetry operations of the jug of Figure 2.2a. We saw that the axis zz is a 2-fold axis to which are associated the two following symmetry operations: rotation by an angle π around zz , which we will denote as A, and the operation A2 or rotation by 2π around zz , which is the identity operation, noted as E. Furthermore, this jug has two other symmetry elements. The plane P going through zz and parallel to the two handles is a symmetry plane or mirror. Let m1 be the operation “symmetry with respect to plane P”. It is clear that m21 = E. In the same way, the plane P going through zz and perpendicular to plane P is a symmetry element. If m2 is the operation “symmetry with respect to plane P ”, then m22 = E. We have thus deﬁned four symmetry operations, viz. A, m1 , m2 and E. We can easily draw the multiplication table for these operations (Tab. 2.1). Table 2.1: Multiplication table for the group of symmetry operations of the jug of Figure 2.2a E

A

m1

m2

E

E

A

m1

m2

A

A

E

m2

m1

m1

m1

m2

E

A

m2

m2

m1

A

E

The product of A and m1 is noted m1 A, the rule being that the order of operations is read from right to left, so that operation A is here followed by operation m1 . This product m1 A is shown at the intersection of line m1 and row A. It is easily checked that this product m1 A is equal to m2 . Consider any point M. The plane perpendicular to the 2-fold axis going through M is

20

Symmetry and Physical Properties of Crystals

represented on Figure 2.6 where uu and vv are the traces, on this plane, of mirrors P and P respectively. v’ (P’ m2) M”

M O

u

u’ (P m1)

M’ v

Figure 2.6: Showing the product of operation A (rotation by π around axis zz perpendicular to the plane of the ﬁgure) and operation m1 (symmetry with respect to the plane P, with trace uu on the ﬁgure). The transform of M through A is M , the transform of M through m1 is M . M is obtained from M through symmetry with respect to plane P , i.e. through operation m2 . We notice that, on each row and each column of the table itself (surrounded by a bold line on Tab. 2.1), all the elements of the group appear, and each appears only once. This is a general result which is derived in Appendix 4A. The generating elements of a group are the elements which are suﬃcient to deﬁne the group. The set of elements of the group is obtained by multiplying these elements with one another or with their inverses. In the example chosen, we see that A and m1 are generating elements of the group, but alternative choices of generating elements are A and m2 or m1 and m2 . A group is said to be commutative if, for any two elements a and b of the group, ab = ba. We see that the group considered above is commutative since the multiplication table is symmetric with respect to its diagonal.

2.4. Exercises Exercise 2.1 We want to derive the following result: if an object has an n-fold axis and a mirror that goes through this axis, it has n mirrors which go through the axis and which enclose between one another angles π/n. 1.

Consider two mirrors, M1 and M2 , enclosing between them an angle α. We note zz the intersection of the two mirrors. Let m1 and m2 be the symmetry operations with respect to plane M1 and to plane M2 respectively. Use a geometrical argument to show that the product m2 m1 is equal to a rotation by 2α around zz , so that m2 m1 = Rotzz (2α).

2.

Deduce from this result that m1 = m2 Rotzz (2α) and m2 = Rotzz (2α)m1 .

Chapter 2 – Symmetry operations

21

3.

Use the result of (2) to obtain the result we seek, viz. that, if an object has an n-fold axis and a mirror that goes through this axis, it has n mirrors deduced from the ﬁrst one through rotations by π/n and its multiples around the axis.

4.

Enumerate the eight symmetry operations of the square-based regular pyramid of Figure 2.2b.

5.

Write down the multiplication table of the group consisting of these symmetry operations. Is it commutative?

Exercise 2.2 Determine the symmetry elements of the two molecules shown below: Br Br

H C

C H

C2 H2 Br2

H H

H C

C

C H

C3 H4

C2 H2 Br2 : the two H atoms and the carbon to which they are linked are coplanar. Their plane is perpendicular to the plane containing the other C atom and the two Br atoms which are linked to it. C3 H4 : the three C atoms are aligned and equidistant. The plane containing the C atom at one end of the chain and the two H atoms which are linked to it is perpendicular to the plane containing the C atom at the other end of the chain and the two H atoms which are linked to it. The angle between the C–H bonds is identical in the two planes. Exercise 2.3 Show that the proper symmetry elements of a cube are: three 4-fold axes, four 3-fold axes and six 2-fold axes.

Chapter 3

Crystal lattices This chapter deﬁnes the crystal lattice, which directly expresses the triple periodicity of the crystal, and all the derived notions: reciprocal lattice, crystal systems and Bravais lattices. The ﬁnal part of the chapter shows how this deﬁnition of the crystal lattice is extended for the study of the surface of crystals.

3.1. Direct lattice We saw that crystals are characterized by their periodicity in three directions. They are deﬁned by a crystal motif consisting of a well-deﬁned set of atoms, which repeats through periodic translations in three non-coplanar directions. We will see that a lattice is associated to this triple periodicity, and that the crystal can thus be deﬁned by its motif and its lattice, which is called direct (in contrast with the so-called reciprocal lattice which will be deduced from the direct lattice in Sect. 3.2).

3.1.1. Unit cell, row Two-dimensional lattice We start with examples of two-dimensional periodic systems because they are easier to represent and to understand, and are well suited for introducing many notions. Figure 3.1a is an example. It shows an elementary motif, a general triangle, periodically reproduced in two diﬀerent directions with period vectors respectively a and b, forming an inﬁnite object. This inﬁnite object features translation symmetry, meaning that any translation t = ua + vb, where u and v are two integers, transforms the object into an object undistinguishable from itself. If we replace the triangle by a group of atoms, we obtain a twodimensional crystal. Now suppose we replace the elementary motif by a point located near the motif in some position, general (i.e. with no special requirement) but perfectly deﬁned with respect to the motif (Fig. 3.1b). We obtain a regular lattice of points which deduce from one another through the set of translations ua + vb

© Springer Science+Business Media Dordrecht 2014 C. Malgrange et al., Symmetry and Physical Properties of Crystals, DOI 10.1007/978-94-017-8993-6_3

23

24

Symmetry and Physical Properties of Crystals

(u and v being integers). This set of points (Fig. 3.1c) is called the crystal lattice, and each point is a lattice node. We can thus deﬁne a plane crystal lattice, with basis vectors a and b, as a set of points M, called nodes, deﬁned by the relation OM = ua + vb where O is any point, chosen as the origin node, and u and v are integers.

b

b

a

a

(b)

(a) M b”

b

a”

a O b’

a’

d

c

(c)

Figure 3.1: (a) A two-dimensional periodic ﬁgure; (b) the associated crystal lattice; (c) examples of primitive cells (a, b), (a , b ), (a , b ) and a multiple unit cell (c, d) Any line going through two nodes is called a row. The parallelogram built on a and b is called the primitive cell for this lattice, and the vectors a and b are its basis vectors. We note that the whole crystal lattice is obtained by paving the whole plane with parallelograms identical to this one, and placing one node at each of the vertices. Each node then belongs to four cells, and counts for 1/4 per cell. One cell then contains 4 times (1/4 node), i.e. one node per cell, and this is why such cells are called primitive cells. It is sometimes designated as a simple unit cell. Vectors a and b are not the only ones which can deﬁne a simple unit cell for a given lattice. Other possible choices are for example the vector pairs a and b , or a and b (Fig. 3.1c). In contrast, vectors c and d deﬁne a cell which also contains a node at its center. The cell is no more a primitive cell, it is termed a multiple cell. Alternative denominations are nonprimitive or centered (or centred) cell. The whole crystal lattice is obtained by setting next to one another such cells, which have a node in common at each of

Chapter 3 – Crystal lattices

25

their vertices and a node at their center. The cell spanning c and d is a double unit cell because it contains two nodes: the node at the center which belongs to only one cell, and the four vertex nodes, each belonging to four cells and counting for 1/4, thus in total another node.1 The number of nodes associated to one unit cell is called the multiplicity or order of the unit cell: thus the cell (c, d) has multiplicity 2. The area of a primitive cell deﬁned by vectors a and b is equal to the norm of the cross product a × b. The areas of all the other primitive cells (such as those deﬁned by a and b or a and b for instance) are identical, each of them being equal to the area associated to one node. The area of a unit cell of order n is equal to n times the area of a primitive cell, since it is equal to the area associated to n nodes. The multiplicity of the cell deﬁned by the vectors f = ua + vb and g = u a + v b (u, v, u , v being integers) can also be determined by computing the cross product f × g: (ua + vb) × (u a + v b) = (uv − u v) (a × b) the norm of which is equal to (uv − u v) a × b, thus an integer (possibly equal to 1) times the area of the primitive cell since u, v, u , v are integers. The crystal lattice is characterized by choosing, if possible, a primitive cell which directly reﬂects the symmetry of the crystal lattice. Suppose for example that the lattice consists of nodes at the vertices of rectangles positioned next to one another (Fig. 3.2a). The lattice is then deﬁned by a rectangular primitive cell, (a, b), and not by a general parallelogram. Now suppose the primitive cell (a, b) of the lattice is a lozenge (Fig. 3.2b). The lattice features symmetry elements: mirrors perpendicular to the plane of the ﬁgure and parallel to the diagonals of the lozenges. These symmetry elements show up immediately if the choice is made of a unit cell with basis vectors c and d, orthogonal to each other, with a node in its center. The lattice is thus deﬁned by a double rectangular cell termed centered rectangular. Three-dimensional lattice The above notions are easily generalized to the case of three-dimensional crystals. The crystal motif is then reproduced through non-coplanar translations a, b, c, and their multiples. Replacing the motif by a point located in some arbitrary but perfectly deﬁned position with respect to the motif produces a regular lattice of points, deduced from one another by translations ua+vb+wc with u, v, w integers. The crystal lattice is then deﬁned by choosing for the origin a point O and drawing all the points M that are the ends of vectors OM = ua + vb + wc with u, v, w integers. The set of points M deﬁnes the crystal lattice and each of these points is called a lattice node. Point O is the origin node.

1. Another way of counting the nodes per unit cell is to imagine the cells to be slightly displaced, so that the lattice nodes no more coincide with the vertices. The nodes in each unit cell are then distinctly visible.

26

Symmetry and Physical Properties of Crystals

b a

d c

b a

(b)

(a)

Figure 3.2: Rectangular plane lattices. The parallelograms built on a and b are primitive cells in both ﬁgures. However, in Figure (a), this parallelogram, actually a rectangle, describes the full symmetry of the lattice. In contrast, describing the symmetry in Figure (b) requires a multiple (centered) unit cell. Any line going through two nodes M and M is called a row, and it contains an inﬁnity of nodes (Fig. 3.3). The vector MM joining nodes M and M has the form u a + v b + w c, where u , v and w are integers since OM and OM are of this form. There is an inﬁnity of rows parallel to MM . The one that goes through the node at origin O goes through node N such that ON = MM = u a + v b + w c. Let u, v and w be integers proportional to u , v and w and mutually prime. The vector ON = ua + vb + wc is the smallest lattice vector parallel to this direction. It deﬁnes the period of the nodes on this row, and more generally on the family of rows parallel to this one, which will be denoted as [uvw].

N’

M’

N

M

O

Figure 3.3: An example of a crystal row. The plane of the ﬁgure is deﬁned by the nodes M and M and the node O taken as the origin.

Chapter 3 – Crystal lattices

27

The parallelepiped spanning the three basis vectors a, b and c is the primitive cell of the crystal (Fig. 3.4a). The sign of the vectors a, b and c is conventionally chosen so that the trihedron a, b, c be direct. The volume of the cell is equal to the mixed product (a, b, c), equal to a · (b × c). We will see that the requirement for a unit cell to feature all the symmetry elements of the crystal lattice leads to deﬁning multiple cells, just as in the case of two-dimensional lattices. Multiple cells can be base-centered if two opposite faces are centered, face-centered if all the faces are centered (Fig. 3.4b), or body-centered if there is a node at the center of the cell. This is why multiple cells are also called centered cells. The multiplicity (or order) of the unit cell is obtained by counting the number of nodes per unit cell, taking into account that a node at the center of the cell adds one node per cell, while a node at the center of a face, belonging to two distinct cells, counts for 1/2.

c1

c

c b b1

b

a a1

a

(a)

(b)

Figure 3.4: (a) Primitive cell of a crystal lattice; (b) multiple, facecentered unit cell with basis vectors a1 , b1 , c1 , and the corresponding primitive cell with basis vectors a, b, c The multiplicity of a cell spanning the crystal lattice vectors a1 , b1 , and c1 such that a1 = u1 a + v1 b + w1 c, b1 = u2 a + v2 b + w2 c, c1 = u3 a + v3 b + w3 c, (ui , vi , wi being integers) can be determined from the volume of the unit cell, equal to the mixed product (a1 , b1 , c1 ). This can be written in matrix from: ⎛

⎞ ⎛ ⎞ a1 a ⎝ b1 ⎠ = U ⎝ b ⎠ c1 c

28 with

Symmetry and Physical Properties of Crystals

⎞ u1 v1 w1 U = ⎝ u2 v2 w2 ⎠ u3 v3 w3 ⎛

Hence (a1 , b1 , c1 ) = det U (a, b, c) where (a, b, c) is the volume of the primitive cell. The multiplicity is thus given by det U .

3.1.2. Lattice planes Any plane that goes through three non-aligned nodes is called a lattice plane. It contains an inﬁnity of nodes, which form a two-dimensional lattice. The set of lattice planes parallel to a given lattice plane describes the whole crystal lattice. In other words, the lattice can be described as the set of the lattice planes of a given family. This can be done in an inﬁnity of ways, since any family of lattice planes can be chosen as the starting point. This is shown on Figure 3.5, based, for simplicity, on a lattice with a primitive cubic cell. The basis vectors a, b and c are therefore mutually orthogonal and have the same length a. The ﬁgure represents the projections of the nodes of this lattice onto a plane perpendicular to one of the basis vectors, for example c. The projected nodes form a square lattice of points, and we have represented the traces of a few families of lattice planes perpendicular to the plane of the ﬁgure. Note, and this is valid whatever the crystal lattice, that the planes of a given family are equally spaced (equidistant) and that the node density in the planes is smaller the closer the planes are to one another.2 Now consider a general crystal lattice, with a primitive cell deﬁned by vectors a, b and c (forming a direct trihedron, as mentioned before). We choose an origin node O and axes Ox, Oy and Oz respectively parallel to a, b and c. We focus on the lattice plane parallel to vector c and containing two nodes M and N belonging to plane (a, b) (Fig. 3.6). The other lattice planes belonging to the same family intersect plane (a, b) along equidistant lines shown dotted on the ﬁgure. One of them goes through the origin O; we label it with number 0. The successive equidistant neighboring planes are numbered 1, 2, 3, . . . , on the side towards which the vectors a and b point, and those located in the other half-space are numbered successively −1, −2, −3, etc. One of these planes necessarily goes through node A, the end of vector a; let h be the integer that characterizes it. In the case shown in the ﬁgure, h = 3, so that it is the third plane. Plane number 1, the one closest to origin, intersects axis Ox at a point with coordinate a/h (a/3 on Fig. 3.6). In the same way, there is necessarily a plane of the same family, numbered k (2 on the ﬁgure), that goes through 2. This is easily veriﬁed by noting that the number n of nodes per unit volume has a given value for a given crystal lattice. On the other hand, on a lattice plane belonging to a given family, the number of nodes per unit area ρ is such that ρ = nd where d is the distance between two successive lattice planes of this family.

Chapter 3 – Crystal lattices

29

node B, the end of vector b. Plane 1 intersects axis Oy at b/k (b/2 on the ﬁgure). Since we chose a family of planes parallel to the basis vector c, plane 1 intersects axis Oz at inﬁnity.

b a

a

Figure 3.5: Projection of a simple cubic lattice on a plane perpendicular to the basis vector c. Various families of lattice planes perpendicular to the plane of the ﬁgure project along the dotted lines. k

y

M B b A O a

x N

−1 0 1 2 3 4

h

Figure 3.6: Traces on plane (a, b) of a family of lattice planes parallel to basis vector c

30

Symmetry and Physical Properties of Crystals

Now let us apply the same reasoning to a general family of lattice planes (Fig. 3.7). The reasoning is based on the fact that a family of lattice planes contains all the lattice nodes, and that all the planes of this family are equidistant. One of these planes, noted P0 , goes through the origin O of the lattice. Another one, called P, goes through the node located at A such that OA = a. There are, between these planes, a number n of equidistant intermediate planes, which divide segment a into an integral number of segments, each with length a/n. Let us call P1 the one which is closest to P0 . y x

z

A

P B a P’ P1 P0

C c Q

b N

M O

P−1

Figure 3.7: A family of lattice planes. P0 is the plane belonging to the family that goes through the origin O of the crystal lattice. P1 and P-1 are the two planes of this family that are closest to O. This plane P1 intersects segment OA at a point M with coordinates (a/h, 0, 0) where h is a positive or negative integer depending on whether plane P1 intersects axis Ox on the side of the positive or negative x, and n = |h|. Similarly, since one of the planes of the family necessarily goes through node B such that OB = b, plane P1 intersects axis Oy at a point N with coordinates (0, b/k, 0) where k is an integer. Finally a plane of the family goes through node C, such that OC = c, and plane P1 intersects axis Oz at Q, with coordinates (0, 0, c/l) where l is an integer. The numbers h, k, l are integers which can be positive or negative. The equation of this plane P1 in the coordinate system Oxyz has the form αx + βy + γz = δ. Writing that the coordinates of M, N and Q satisfy this equation, we obtain: b c a = δ, β = δ, γ = δ. h k l Replacing α, β and γ by their values as a function of δ, the equation of plane P1 becomes x y z h + k + l = 1. a b c α

Chapter 3 – Crystal lattices

31

Let us select as the length unit on each of the axes the length of the corresponding basis vector, viz. a on Ox, b on Oy and c on Oz, and this is the choice we will use throughout this book, this equation becomes hx + ky + lz = 1.

(3.1)

The equation of the n-th plane of this family, on the same side as P1 with respect to the origin, is hx + ky + lz = n while the n-th plane on the other side is hx + ky + lz = −n. The equation of the plane belonging to this family and going through the origin is hx + ky + lz = 0. (3.2) The integers h, k and l are mutually prime. Let us show this by supposing they were not. Then we could write h = mh , k = mk and l = ml where m, h , k and l are integers. Equation (3.1) would then become 1 . m It must be satisﬁed by all the nodes of the plane, the coordinates of which are integers. h , k and l being integers, this is impossible if m = 1 since then 1/m would not be an integer. h x + k y + l z =

This family of lattice planes is designated as (hkl) and we will remember that: The notation (hkl), where h, k and l are mutually prime integers, designates a family of lattice planes such that the plane of the family closest to the node at origin intersects axis Ox at a/h, axis Oy at b/k and axis Oz at c/l. h, k and l are called the Miller indices of this family of lattice planes. Note that the integers h, k and l are placed between parentheses while the integers deﬁning a family of rows (Sect. 3.1.1) are noted between square brackets. Note: the planes parallel to a have the designation (0kl) since they intersect axis Ox at inﬁnity. Similarly the planes parallel to b have the form (h0l) and those parallel to c the form (hk0). Application: what condition must h, k, l and u, v, w satisfy for a plane (hkl) and a row [uvw] to be parallel to each other? Row [uvw] is by deﬁnition parallel to the vector OM = ua + vb + wc. The plane parallel to the row and going through origin therefore contains the point M, with coordinates u, v, w and, from (3.2), we must have hu + kv + lw = 0. We note that: A row [uvw] is parallel to a plane (hkl) if and only if hu + kv + lw = 0.

32

Symmetry and Physical Properties of Crystals

3.1.3. Wigner-Seitz cell Solid-state physicists often use another way of subdividing direct space into identical cells containing one lattice node per cell. The center of these cells is chosen on one lattice node. The mediating planes of the segments joining the chosen node to the ﬁrst nodes on the various rows which point out of this node are then drawn. The smallest volume thus created around the node is the Wigner-Seitz cell (Fig. 3.8). This cell is primitive because it is associated to a single lattice node, but it is not a parallelepiped. In Section 3.2, we will deﬁne another lattice of points, deduced from the direct lattice, which is called the reciprocal lattice. The same construction applied to this reciprocal lattice deﬁnes a cell called the ﬁrst Brillouin zone.

Figure 3.8: Wigner-Seitz cell of a plane lattice. The segment in dotted lines connects the origin to a node which does not take part in the construction of the cell because the mediator of this segment is outside the cell.

3.2. Reciprocal lattice 3.2.1. Introduction based on diﬀraction The above considered lattice is deﬁned in the space of the crystal, and this is why it is called the direct lattice. Another associated lattice is very much used: it is called the reciprocal lattice and plays a part in the phenomena of diﬀraction by crystals and more generally in all problems of wave propagation in crystals. It is the space of wave vectors, the dimensions of which are reciprocal lengths. It should be mentioned that the crystallographers’ tradition is to write a plane wave w, with amplitude a and frequency ν (angular frequency ω = 2πν) in the form w = a cos 2π(k · r − νt), so that the norm of the wave-vector is equal to 1/λ where λ is the spatial period of the wave, i.e. the wavelength. This is in contrast with the tradition of optics and of most physicists, who write w = a cos(k · r − ωt), so that the norm of their k is equal to 2π/λ. This is summarized in Table 3.1 below. The triple periodicity in the position of atoms in a crystal leads to a plane wave of monochromatic X-rays incident on the crystal being diﬀracted into well-deﬁned directions.

Chapter 3 – Crystal lattices

33

Table 3.1: Deﬁnition of the wave-vector k as used in various areas of physics Crystallography

w = a cos 2π(k · r − νt) ||k|| = 1/λ

Optics, quantum mechanics, solid state physics

w = a cos(k · r − ωt) ||k|| = 2π/λ

Consider a crystal whose primitive cell is deﬁned by the vectors a, b and c. This crystal consists in a motif and its transforms by all the translations of the crystal lattice τ = ua + vb + wc (u, v, w integers). Let ko be the wave-vector of the incident wave. This wave interacts with the electrons in the atoms of the crystal motif. Assume for simplicity that the motif consists of a single atom. This monoatomic motif scatters into all space a spherical wave with the same wavelength. For an observer located far enough from the crystal, this spherical wave can be considered as plane with a wave-vector kd . The waves scattered by two identical motifs located at P and Q, a vector τ = ua + vb + wc apart, have a path diﬀerence δ = PK − HQ such that: δ = (sd − so ) · τ where sd and so are unit vectors along kd and ko respectively. sd K

so

P ko

H

kd Q

Figure 3.9: Scattering of a plane wave by two crystal motifs separated by a vector τ All the plane waves scattered by all the motifs are in phase if δ = nλ (n an integer) for all τ , so that (sd − so ) · τ = nλ or

(kd − ko ) · τ = n

(3.3)

since |kd | = |ko | = 1/λ. This is seen to involve calculating the dot product of a vector τ of direct space, expressed in a non-orthonormal basis {a, b, c}, and a vector of the space of wave-vectors. This dot product is easily written if the vector kd − ko is expressed in a basis {a∗ , b∗ , c∗ } such that the dot product of a∗ and a is equal to 1 while the dot products of a∗ and b or c are zero, with similar

34

Symmetry and Physical Properties of Crystals

relations for b∗ an c∗ : a∗ · a = 1

a∗ · b = 0

a∗ · c = 0

∗

b∗ · b = 1

b∗ · c = 0

∗

c∗

b · a=0 c · a=0

· b=0

(3.4)

∗

c · c=1

Let u∗ , v ∗ and w∗ be the components of the vector kd − ko in the basis {a∗ , b∗ , c∗ }. The vector kd − ko is expressed as kd − ko = u∗ a∗ + v ∗ b∗ + w∗ c∗ . Taking into account Equations (3.4), condition (3.3), with n an integer, takes the form u∗ u + v ∗ v + w ∗ w = n which must be veriﬁed for all integral values of u, v and w. This requires that u∗ , v ∗ and w∗ be integers. The reciprocal lattice of a crystal is deﬁned as the set of points N obtained starting from an origin O and such that ON = ha∗ + kb∗ + lc∗ where h, k and l are integers. The points N are the nodes of the reciprocal lattice and O the origin node. We just showed that the diﬀraction condition is equivalent to the condition that the components u∗ , v ∗ and w∗ , in the basis of the reciprocal lattice, of the scattering vector (or diﬀraction vector) kd − ko be integers, i.e. that this scattering vector be a vector joining two nodes of the reciprocal lattice. The diﬀraction condition is thus very simply expressed thanks to the reciprocal lattice. Furthermore, we see on Equations (3.4) that: The reciprocal lattice of the reciprocal lattice is the direct lattice. This results from the fact that the ﬁrst column of Equations (3.4) deﬁnes a as a function of a∗ , b∗ and c∗ just like the ﬁrst row deﬁnes a∗ as a function of a, b and c, etc.

3.2.2. Alternative deﬁnition of the reciprocal lattice The relations (3.4) show that a∗ is perpendicular to b and c, hence parallel to the cross product b × c. We can thus write: a∗ = α (b × c). Furthermore, since a · a∗ = 1, we have: a · a∗ = α a · (b × c) = αv0 = 1, with v0 = (a, b, c) the volume of the crystal unit cell. Hence α = 1/v0 and therefore a∗ = (b × c)/v0 .

Chapter 3 – Crystal lattices

35

In the same way, we obtain b∗ = (c × a)/v0 , and

c∗ = (a × b)/v0 .

(3.5)

Relations (3.5) directly deﬁne the reciprocal lattice with respect to the basis vectors of the direct lattice. This is the most usual deﬁnition of the basis vectors of the reciprocal lattice. Further, since the direct lattice is the reciprocal lattice of the reciprocal lattice, a = (b∗ × c∗ )/v0∗ , b = (c∗ × a∗ )/v0∗ , c=

(a∗

×b

∗

(3.6)

)/v0∗ ,

with v0∗ the volume of the reciprocal unit cell, i.e. the volume of the parallelogram built on a∗ , b∗ and c∗ .

3.2.3. Properties of the reciprocal lattice Basic property Consider the lattice plane P1 of the family (hkl) that is closest to the origin O of the direct lattice. A point M of this plane has coordinates x, y, z in basis {a, b, c}: OM = xa + yb + zc. From relation (3.1), x, y and z then satisfy the relation hx + ky + lz = 1

(3.7)

where we recall that the integers h, k and l are mutually prime. Consider the vector h∗ of the reciprocal lattice with components h, k and l h∗ = ha∗ + kb∗ + lc∗ . The properties of the reciprocal lattice encountered above show that OM · h∗ = hx + ky + lz and, taking into account (3.7), OM · h∗ = 1. Let H be the projection of M on the vector h∗ (Fig. 3.10), with norm ||h∗ || . OM · h∗ = OH ||h∗ || = 1 and

OH = 1/|| h∗ || = constant.

36

Symmetry and Physical Properties of Crystals

H M

P1 dhkl h* O P0

Figure 3.10: Two neighboring (hkl ) planes: P0 goes through the origin of the lattice and P1 is its ﬁrst neighbor. We deduce that all points of plane P1 project onto vector h∗ at the same point H, which means that plane P1 is perpendicular to the vector h∗ . On the other hand, OH is the distance of plane P1 to the plane of the family (hkl) which goes through O. This is the distance dhkl between two successive planes in the family (hkl). We thus obtain dhkl =

1 . ||h∗ ||

(3.8)

Basic property: The planes (hkl) are perpendicular to the row [hkl]∗ of the reciprocal lattice and their distance dhkl is equal to the reciprocal of the modulus of the vector h∗ = ha∗ + kb∗ + lc∗ . It is important to recall that the vector h∗ which is being discussed as a way of calculating the distance between two neighboring lattice planes of family (hkl) connects the origin of the reciprocal lattice3 to the ﬁrst reciprocal lattice node on the row [hkl]∗ that goes through the origin, since h, k, l are mutually prime. X-ray diﬀraction can also be described in terms of selective mirror reﬂection of X-rays on the lattice planes. The condition for constructive interference is given by Bragg’s law 2dhkl sin θ = nλ where λ is the wavelength, θ the complement of the angle of incidence on the lattice planes, and n the order of the reﬂection. Bragg’s law can also be written 2(dhkl /n) sin θ = λ and the reﬂection of order n on the lattice planes (hkl) described by arbitrarily introducing reﬂecting planes parallel to the lattice planes (hkl), and n times closer to one another, their distance being dhkl /n. This distance dhkl /n between reﬂecting planes is equal to 1/(n||h∗ ||), i.e. the reciprocal of the norm of a new vector h∗ = nh∗ of 3. For simplicity, we select the origin of the reciprocal lattice as coinciding with that of the direct lattice.

Chapter 3 – Crystal lattices

37

the reciprocal lattice connecting the origin of the reciprocal lattice to the n-th node on the row [hkl]∗ . One then speaks of a reﬂection nh, nk, nl such that 2dnh,nk,nl sin θ = λ with dnh,nk,nl = 1/||h∗ || where h∗ is now the reciprocal lattice vector connecting the origin to the n-th node along row [hkl]∗ . In this way each reciprocal lattice node is associated to a reﬂection, the ﬁrst node in each row corresponding to the reﬂection of order 1 and the n-th node to the reﬂection of order n. We note that everything concerning the reciprocal lattice is indicated by a star: the basis vectors a∗ , b∗ , c∗ , a row [hkl]∗ and a family of lattice planes (hkl)∗ . Since the lattice reciprocal to the reciprocal lattice is the direct lattice, we can similarly state that: The planes (hkl)∗ of the reciprocal lattice are perpendicular to the row [hkl] of the direct lattice. Volume of the reciprocal unit cell Let us substitute, in the expression (3.5) for a∗ , the vector c by its expression (3.6) as a function of the reciprocal lattice vectors. We obtain a∗ = (b × (a∗ × b∗ ))/v0 v0∗ . Using the expression of the double cross product A × (B × C) = B (A · C) − C (A · B), and relations (3.4), we obtain a∗ = [a∗ (b · b∗ ) − b∗ (b · a∗ )]/v0 v0∗ = a∗ /v0 v0∗ . This shows that

v0 v0∗ = 1.

(3.9)

Note: all of the above discussion refers to unit cells associated with a single lattice node (primitive cells). The reciprocal lattice of a multiple unit cell must be deﬁned using a primitive cell. It is however possible to then describe the reciprocal lattice using a multiple reciprocal unit cell (see Sect. 3.7.3).

3.2.4. Crystallographic calculations Calculation of lattice distances The lattice distance dhkl in a family of lattice planes (hkl) is determined by relation (3.8), which yields: 1 = (ha∗ + kb∗ + lc∗ )2 , d2hkl where the basis vectors a∗ , b∗ and c∗ of the reciprocal lattice are determined as a function of the basis vectors a, b and c of the direct lattice through relations (3.5).

38

Symmetry and Physical Properties of Crystals

We thus obtain 1 = (ha∗ + kb∗ + lc∗ )2 d2hkl = h2 a∗2 + k 2 b∗2 + l2 c∗2 + 2hk a∗ · b∗ + 2kl b∗ · c∗ + 2lh c∗ · a∗ . (3.10) In Section 3.4.2, we will deﬁne the crystal systems, and derive the expressions for the values of dhkl in each of them. Search for the indices of a lattice plane parallel to two rows of the direct lattice We are looking for the plane (hkl) which is parallel to rows [u1 v1 w1 ] and [u2 v2 w2 ]. First method: We saw, at the end of Section 3.1.2, that the condition for row [uvw] of the direct lattice to be parallel to plane (hkl) is that hu + kv + lw = 0.

(3.11)

We apply this condition to both rows: hu1 + kv1 + lw1 = 0, hu2 + kv2 + lw2 = 0. We deduce that k l h = = . v1 w2 − w1 v2 w1 u2 − u1 w2 u1 v2 − v1 u2

(3.12)

Second method: Let n1 = u1 a + v1 b + w1 c and n2 = u2 a + v2 b + w2 c be vectors parallel to the two rows respectively. The plane we are looking for, being parallel to both vectors, is perpendicular to the cross product of the vectors n1 and n2 , which is expressed as n1 × n2 = (u1 a + v1 b + w1 c ) × (u2 a + v2 b + w2 c) = (v1 w2 − w1 v2 )(b × c) + (w1 u2 − u1 w2 )(c × a) + (u1 v2 − v1 u2 )(a × b).

(3.13)

Taking into account Equations (3.5) which deﬁne the basis vectors of the reciprocal lattice, we obtain: n1 × n2 = v0 [(v1 w2 − w1 v2 )a∗ + (w1 u2 − u1 w2 )b∗ + (u1 v2 − v1 u2 )c∗ ].

(3.14)

Chapter 3 – Crystal lattices

39

We see that The cross product of two vectors of direct space lattice is parallel to a vector of the reciprocal lattice, a result which will be used in the next paragraph. Let us write the cross product (3.14) in the following form: n1 × n2 = v0 [h a∗ + k b∗ + l c∗ ] where h = v1 w2 − w1 v2 , k = w1 u2 − u1 w2 and l = u1 v2 − v1 u2 are integers since ui , vi and wi are integers. If h , k , l are not mutually prime, call h, k, and l the mutually prime integers proportional to them (h = nh, k = nk, l = nl). Thus n1 × n2 is parallel to the vector [hkl]∗ of the reciprocal lattice, with h, k and l mutually prime. Such a vector is perpendicular to the plane (hkl) of the direct lattice, which is the plane we are looking for. We thus retrieve relations (3.12). Search for the row [uvw] parallel to the intersection of planes (h1 k1 l1 ) and (h2 k2 l2 ) First method: We apply condition (3.11) to the row [uvw] and to the planes (h1 k1 l1 ) and (h2 k2 l2 ). h1 u + k1 v + l1 w = 0, h2 u + k2 v + l2 w = 0. We deduce that v w u = = . k1 l2 − l1 k2 l1 h2 − h1 l2 h1 k2 − k1 h2

(3.15)

Second method: The vectors V∗1 = h1 a∗ + k1 b∗ + l1 c∗ and V∗2 = h2 a∗ + k2 b∗ + l2 c∗ are perpendicular to the planes (h1 k1 l1 ) and (h2 k2 l2 ) respectively. The row we are looking for is therefore perpendicular to these vectors, hence parallel to the cross product V∗1 × V∗2 . The latter is parallel to a vector of the space reciprocal to reciprocal space, i.e. a vector of direct space. Following the same approach as in (3.13) and (3.14), we obtain: V∗1 × V∗2 = v0∗ [(k1 l2 − l1 k2 ) a + (l1 h2 − h1 l2 ) b + (h1 k2 − k1 h2 ) c] and we retrieve the result (3.15).

40

Symmetry and Physical Properties of Crystals

3.3. Properties of crystal lattices 3.3.1. Centers of symmetry All nodes of a crystal lattice are centers of symmetry for the lattice, as we can easily see, for example on the two-dimensional lattice of Figure 3.1c. The same applies to the centers of the unit cells. Therefore All crystal lattices feature centers of symmetry.

3.3.2. n-fold and n ¯ -fold axes consistent with the crystalline state We will now show that: A crystal lattice can only feature n-fold axes of order 2, 3, 4 or 6. The same applies to n ¯ -fold axes, which can only be 1¯ , 2¯ , 3¯ , 4¯ or 6¯ axes. First derivation: Consider a vector V of the crystal lattice. If the lattice features a symmetry element, one of the symmetry operations S associated to this element will transform V into a vector V = SV which is also a lattice vector. V and V , being lattice vectors, have integral components with respect to the coordinate system deﬁned by the basis vectors a, b and c of the crystal unit cell. The coeﬃcients in the matrix representing operation S in this basis are therefore integers, and its trace is also an integer. If a lattice features an n-fold axis, let us call S the rotation by α = 2π/n around this axis, denoted An . The trace of the matrix representing an operator does not depend on the basis chosen (orthonormal or not) to represent this operator. We choose to represent this operator in an orthonormal frame such that Oz coincides with axis An hence through matrix S ⎛ ⎞ cos α − sin α 0 S = ⎝ sin α cos α 0 ⎠ . 0 0 1 The trace of S is equal to 1 + 2 cos α: therefore 2 cos α must be an integer. Furthermore, |2 cos α| ≤ 2 and the only possible values of 2 cos α are therefore: −2, −1, 0, 1, 2. If cos α = ±1, α = 0 or π. There is a 1-fold axis, i.e. no symmetry (if α = 0), or a 2-fold axis (if α = π). If cos α = ±1/2, α = ±2π/3 or ±π/3, and there is a 3-fold axis or a 6-fold axis. If cos α = 0, α = ±π/2 and there is a 4-fold axis. The only possible values for n are therefore n = 1 (trivial), 2, 3, 4 and 6.

Chapter 3 – Crystal lattices

41

The derivation is the same for the n ¯ axes. Operation S is then the rotation by α = 2π/n followed by an inversion with respect to a center located on the rotation axis. The matrix representing this operation is then −ES where S is the above matrix and E is the unit matrix. The trace of this matrix is −(1 + 2 cos α), which must be an integer; therefore 2 cos α is an integer with modulus less or equal to 2. We thus retrieve the preceding results, hence the same consequences, viz. the possible existence of ¯1, ¯2, ¯3, ¯4 and ¯6 axes. A ¯1 axis is identical to a symmetry center, already mentioned in Section 3.3.1. Second (geometrical) derivation This derivation applies more conveniently to rotation axes. We use the result, independently derived in Section 3.3.4 below, that an n-fold axis is perpendicular to a family of lattice planes, hence to a set of lattice vectors. Let V = AB be an elementary vector of the crystal lattice (i.e. a vector connecting two neighboring nodes), perpendicular to the n-fold axis. Let us perform onto AB the symmetry operation S, a rotation by α = 2π/n around the n-fold axis that goes through node A (Fig. 3.11). The vector AB becomes AB , which therefore is a lattice vector. Operation S, performed n − 1 times, is a symmetry operation. It is a rotation by (n − 1)α = 2π − α = −α (modulo 2π). We recall that two angles are equal modulo 2π if their diﬀerence is an integer times 2π. Let us apply this rotation −α to vector AB using the axis located at B:4 BA becomes BA , a lattice vector. It is easy to show that vector B A is parallel to AB. Its length is equal to AB(1 − 2 cos α) and it is a lattice vector. It is therefore equal to an integer times AB. Thus (1 − 2 cos α) is an integer and 2 cos α is an integer. We retrieve the same results as above. A’

B’

A

– B

Figure 3.11: A and B are two neighboring nodes on a crystal lattice featuring n -fold axes perpendicular to the plane of the ﬁgure.

3.3.3. The direct lattice and the reciprocal lattice have the same symmetry elements Let S be a symmetry operation (rotation or rotoinversion) featured by a given direct crystal lattice. It therefore transforms the direct lattice R into a lattice R with which it is superimposed, so that SR = R ≡ R.

4. Translation symmetry implies the existence of an n-fold axis at B if there is one at A.

42

Symmetry and Physical Properties of Crystals

Let a , b and c be the transforms of a, b and c under S. We can write a = S a,

b = S b and c = S c.

The reciprocal lattice R∗ of R can be obtained from a , b and c or from a, b and c since R and R are identical. We want to show that the symmetry operation S transforms R∗ into itself. Let us deﬁne R∗ through a∗ , b∗ and c∗ such that: a∗ = (b × c )/v0 = (Sb × Sc)/v0 = ±S(b × c)/v0 = ±Sa∗ = S(±a∗ ). Similarly, b∗ = S(±b∗ ) and c∗ = S(±c∗ ). The sign + or − depends on the nature (proper or improper) of S but R∗ can be deﬁned using −a∗ , −b∗ and −c∗ just as well as using a∗ , b∗ and c∗ . We therefore see clearly that the lattice R∗ is transformed by S into itself. S is thus a symmetry operation for the reciprocal lattice.

3.3.4. Geometrical relation between the symmetry axes and the crystal lattice We now show that: Any symmetry axis (rotation or rotoinversion axis) is parallel to a row of the direct lattice and perpendicular to a lattice plane. Let S be the elementary symmetry operation associated to the n-fold axis (rotation by 2π/n) or n ¯ −fold axis (rotation by 2π/n followed by an inversion). It transforms a vector V parallel to the axis into an equal (rotation case) or opposite (rotoinversion case) vector. SV = ±V

or

(S ∓ E)V = 0

where E is the unit operator. In the basis a, b, c, the coeﬃcients of the matrix S representing operation S are integers since S transforms a lattice vector into another lattice vector. The same applies to S ± E. Solving the equation system (S ± E)V = 0, we ﬁnd that the components u, v and w of vector V are such that u/w = p/r and v/w = q/r with p, q and r integers, whence u/p = v/q = w/r. Since p, q and r are integers, the symmetry axis is parallel to a row5 [p q r] of the lattice. The same derivation can be applied to the reciprocal lattice, which also features this symmetry element (Sect. 3.3.3). The symmetry axis is thus also parallel to a reciprocal lattice row, and thus perpendicular to a lattice plane of the direct lattice (see Sect. 3.2.3). 5. The integers p, q and r are not necessarily mutually prime. If they are not, they should be replaced by numbers proportional to p, q and r and mutually prime, in order to deﬁne the row adequately.

Chapter 3 – Crystal lattices

43

3.3.5. The lattice is at least as symmetrical as the crystal Pierre and Jacques Curie stated in 1894 a very far-reaching principle which is now called the Curie principle. It will be introduced in Chapter 9 (Sect. 9.5.2) and widely used in the second part of this book. One of the direct consequences of this principle can be stated as follows: the physical properties of a crystal are at least as symmetrical as the crystal. The crystal lattice describes one property of the crystal, viz. its triple periodicity. Therefore the crystal lattice must be at least as symmetric as the crystal. This property will be derived in Section 4.2.3 and used in Section 5.6 to determine the crystal lattice of a crystal as a function of the symmetry properties of the crystal itself.

3.4. Crystal systems The results mentioned in this section are not derived but the enumeration of crystal systems introduced below is so natural that it can be performed before their precise deﬁnition is introduced (Sect. 5.6 and Chap. 6). Suﬃce it to say that a crystal system is characterized by the smallest unit cell, primitive or multiple (centered), which features all the symmetry elements of the corresponding lattice.

3.4.1. Two-dimensional crystal systems Let us recall that the symmetry elements of a plane object are perpendicular to the plane of the object, and that a center of symmetry O is then equivalent to a 2-fold axis perpendicular to the plane and going through O. There are four plane crystal systems, shown in Table 3.2. Table 3.2: The plane crystal systems System Unit cell shape

Oblique

Rectangular

Square

Hexagonal

parallelogram

rectangle

square

lozenge with angle 120° 120°

Bravais lattices

p

p c (centered)

p

p

They are: the oblique (general primitive cell), rectangular (rectangular primitive cell), square (square primitive cell), and hexagonal (primitive cell in the shape of a lozenge with angle 120◦ ) systems. We note that a lozenge-shaped primitive cell produces a rectangular centered lattice. The rectangular centered double cell evidences more explicitly the symmetry elements of the lattice,

44

Symmetry and Physical Properties of Crystals

viz. the mirror symmetry planes parallel to the basis vectors of the centered rectangular cell. We will see (Sect. 3.7) that they are the primitive (p) and centered (c) Bravais lattices.

3.4.2. Three-dimensional crystal systems There are seven three-dimensional crystal systems, deﬁned and illustrated in Table 3.3. The basis vectors of the unit cell are always called a, b, c and the trihedron a, b, c is chosen as direct. The angles in the cell faces are denoted as α = (b, c), β = (c, a) and γ = (a, b). The seven systems are the following: Triclinic: the unit cell is a general parallelepiped, deﬁned by its three angles α, β, and γ (in Greek, klinos means angle) and the lengths a, b and c of the three basis vectors. Monoclinic: the unit cell is a right prism with bases in the shape of a parallelogram, deﬁned by just one angle (whence the name) since the two others are right angles, and the lengths a, b and c of the three basis vectors. The basis vector perpendicular to the two others was long selected as the vector b, and the angle to be deﬁned is then β. Nowadays a frequent choice, more consistent with the choices for the other systems, is to take it as vector c, and the angle to be deﬁned is then angle γ. Orthorhombic (from the Greek orthos = right): the unit cell is a rectangle parallelepiped. All that is to be deﬁned are the three lattice parameters a, b and c. Tetragonal: the unit cell is a right prism with square base (a rectangle parallelepiped in which two opposite faces are square). One chooses to call a and b the basis vectors forming the square and c the basis vector which is perpendicular to them. Two lattice parameters must therefore be deﬁned: a = b and c. Rhombohedral (or trigonal): the unit cell is a rhombohedron, i.e. a parallelepiped in which all the faces are equal (Fig. 3.14a). The only values to be deﬁned are the lattice parameter a = b = c and the angle α = β = γ. We can visualize a rhombohedron as a cube which has been drawn out or compressed along one of its major diagonals. In a cube, the major diagonals are 3-fold axes. If a cube is drawn out or ﬂattened along one of its major diagonals while retaining the equality of the edges, this diagonal remains a 3-fold axis while the others are no longer 3-fold axes. The rhombohedral lattice is described in more detail in Section 3.6.2. Hexagonal: the unit cell is a special right prism. Its base is a lozenge with one angle equal to 120◦ . The basis vector perpendicular to the two others is c. Two cell parameters must be deﬁned: a = b and c. Cubic: the unit cell is a cube, and the only parameter to be deﬁned is a = b = c.

Chapter 3 – Crystal lattices

45

Table 3.3: The seven three-dimensional crystal systems Crystal system Shape of unit cell

Parameters

Polyhedron

Bravais lattices

Triclinic

a b c

general parallelepiped

P

c b

c

Monoclinic

a a b c general

b

a a b c general

b a c

Orthorhombic

cb

P, A (or B) right prism with parallelogram-shaped base P, C (or A)

a b c

right prism with rectangular base

P A (or B or C) I, F

a b c

right prism with square base

P, I

a b c

rhombohedron

R (P)

a b c 120°

right prism with 120° lozenge base

P

a b c

cube

P, I, F

a

Tetragonal

c

b a

Rhombohedral (Trigonal) ab

c

Hexagonal b

Cubic

c a

cb a

46

Symmetry and Physical Properties of Crystals

In each crystal system, the lattice distance dhkl can be calculated as a function of the basis vectors a∗ , b∗ and c∗ of the reciprocal lattice using formula (3.10). For all systems except for the triclinic and rhombohedral systems, this formula can be simpliﬁed, and dhkl is easily expressed as a function of the parameters of the direct lattice, i.e. of the lengths a, b and c of the basis vectors and the angles α, β and γ between these vectors. Some of these calculations are the topics of exercises, and the result for the various crystal systems is given in Table 3.4. For the triclinic and rhombohedral lattices, it is convenient to use a quantity called the metric tensor, which is introduced in Appendix 3A. The metric tensor is widely used in numerical calculations for crystallography. Table 3.4: Lattice distances for the various crystal systems dhkl

Crystal system

Triclinic Monoclinic

Orthorhombic

1 − cos2 α − cos2 β − cos2 γ + 2 cos α cos β cos γ A 2 2 h2 hl sinβ / + cl 2 + kb sin2 β − 2 ac cos β a2 if b // 2-fold axis of the cell l 2 2 h2 k2 sinγ / sin γ − 2 hk ab cos γ a2 + b2 + c if c // 2-fold axis of the cell 2 1 / ha2 +

k2 b2

+

l2 c2

Rhombohedral

2 a / h2 + k 2 + l2 ac 1+2 cos3 α−3 cos2 α a 2 2 2 2

Hexagonal

2 a / 43 (h2 + k 2 + hk) + l2 ac

Cubic

√ a / h2 + k 2 + l2

Tetragonal

(h +k +l ) sin α+2(hk+kl+lh)(cos2 α−cos α)

h2 k2 l2 hk 2 2 sin α + sin β + sin2 γ + 2 (cos α cos β − cos γ) 2 2 2 a b c ab kl hl + 2 (cos α cos γ − cos β) + 2 (cos β cos γ − cos α) ac bc

A=

Chapter 3 – Crystal lattices

47

3.5. Examples of reciprocal lattices 3.5.1. Monoclinic lattice The unit cell is deﬁned by the lengths a, b, c of the basis vectors and by the angle β between vectors a and c (if the choice is to denote as b the basis vector parallel to the 2-fold axis of the cell). The volume v0 of the unit cell is equal to abc sin β. b×c v0 c ×a b∗ = v0 a×b ∗ c = v0 a∗ =

and and and

1 ; a sin β 1 b∗ = ; b 1 ∗ c = . c sin β

a∗ =

Vector b∗ is parallel to vector b. The vectors a∗ and c∗ are in the plane of vectors a and c and perpendicular to c and a respectively. The angle between a∗ and c∗ is equal to π − β (Fig. 3.12). The hexagonal lattice can be treated the same way (Exercise 3.4). a

a*

9

b,b*

c* c

Figure 3.12: Basis vectors of a monoclinic lattice and of the corresponding reciprocal lattice projected on a plane perpendicular to vector b (parallel to the 2-fold axis). The vectors b and b∗ are perpendicular to the plane of the ﬁgure and point upwards.

3.5.2. Orthorhombic, tetragonal and cubic lattices In these three lattices, the basis vectors a, b and c are mutually orthogonal: therefore the vectors a∗ , b∗ and c∗ are parallel to vectors a, b and c respectively, and their lengths a∗ , b∗ and c∗ are equal to 1/a, 1/b and 1/c respectively. In the tetragonal lattice, a = b and a∗ = b∗ . In the cubic lattice where a = b = c, the three basis vectors of the reciprocal lattice have the same length a∗ = b∗ = c∗ = 1/a.

48

Symmetry and Physical Properties of Crystals

3.6. Hexagonal lattice and rhombohedral lattice 3.6.1. Hexagonal lattice The hexagonal lattice is deﬁned from two basis vectors a and b with the same length, enclosing an angle of 120◦ (Fig. 3.13), and a vector c perpendicular to a and b. In the basal plane deﬁned by the vectors a and b, we could just as well select the vector couples b and d (or d and a) where d is the vector deduced from b through a rotation by 120◦ around the 6-fold axis of the lattice (parallel to c). These three vectors a, b and d are related by: a + b + d = 0.

b d

a

Figure 3.13: Hexagonal lattice; projection of the nodes onto a plane perpendicular to c To evidence, in the lattice plane notation, the 3-fold symmetry of these vectors, a fourth index i is added between indices k and l, leading to the notation (hkil) such that the lattice plane closest to origin intersects the vectors a, b, d and c at a/h, b/k, d/i and c/l. It can be shown (Exercise 3.5) that the relation h+k+i=0

or

i = −(h + k)

applies. This four-index notation makes it possible to easily determine the lattice planes equivalent through the symmetry operations of the crystal (Exercises 3.5 and 5.6). The notation (hkil) is sometimes replaced by (hk.l) to show that one deals with a hexagonal lattice. This four-index notation cannot apply to rows [uvw], since it is then meaningless.

3.6.2. Rhombohedral lattice Consider a rhombohedral lattice. The unit cell is a rhombohedron shown on Figure 3.14a. Its basis vectors are LP = a, LM = b and LN = c. The plane MNP is a (111) plane, noted as Π1 on Figure 3.14b. We note as Π0 the (111) plane containing node L, Π2 the one containing nodes Q, R and S and Π3 the one containing T.

Chapter 3 – Crystal lattices

49 T

T 3 R

R

S

Q

N c

P a

M

2

S

N 1

R’

Q

L

M L’

P

M

S’#

B& P

(a)

& #

N

b 0

&

#

& #Q’

A

#

J

L

(b)

(c)

Figure 3.14: Rhombohedral lattice: (a) primitive cell; (b) showing the succession of (111) planes; (c) projection of the lattice onto plane Π1 , perpendicular to the 3-fold axis (empty circles for the nodes of Π0 and Π3 , full circles for the nodes of Π1 , and crosses for the nodes of Π2 ) The nodes in each of these (111) planes form a hexagonal plane lattice since they are at the vertices of adjacent equilateral triangles. The nodes of planes Π0 (containing L) and Π3 (containing T) project onto Π1 at L , the center of triangle MNP, and on all equivalent points (empty circles in Fig. 3.14c), i.e. at the centers of every other of the equilateral triangles formed by the hexagonal plane lattice of Π1 . The nodes of plane Π2 such as Q, R and S project at the centers of the other triangles (crosses, and for example Q , R and S , the projections of Q, R and S respectively). We immediately see on Figure 3.14c that the rhombohedral lattice can be described by a triple hexagonal unit cell, with basis vectors A = PJ = NM = NL + LM = b − c, B = PN = PL + LN = c − a, C = LT = LN + NR + RT = a + b + c, so that ﬁnally

A = b − c, B = c − a, C = a + b + c.

This unit cell is triple because it contains the nodes Q and T which project onto Π1 at Q and L respectively. We can add to the basis vectors A and B a vector D deﬁned as in Section 3.6.1, i.e. such that A+B+D=0 so that D = MP = a – b.

50

Symmetry and Physical Properties of Crystals

It is current practice to describe a rhombohedral lattice in this way, through its triple hexagonal unit cell, with basis vectors A, B and C, because it is much easier to handle. Conversely, the basis vectors of the rhombohedral unit cell are obtained from those of the hexagonal unit cell through the relations C D−B + , 3 3 C A−D b= + , 3 3 C B−A c= + . 3 3 a=

3.7. Bravais lattices 3.7.1. Why they are needed We are not going to systematically enumerate the Bravais lattices. This will be done in Chapter 6. Here we introduce them after showing why it is of interest to deﬁne them. In many cases, the primitive cell considered as an individual object has symmetry lower than the symmetry of the lattice, while a multiple (or centered) cell can evidence the symmetry of the lattice. A ﬁrst example is the case of a rhombohedral unit cell with angle equal to 60◦ . When the whole lattice is represented, we ﬁnd that the nodes are at the vertices of cubes and at the centers of the faces of these cubes (Fig. 3.15a). The derivation is simpler when starting from the face-centered cubic (fcc) lattice. It is then easy to see that the parallelepiped in which the basis vectors A, B, C connect a vertex P to the centers Q, R, S of the faces starting in P is a rhombohedron with apical angle 60◦ , since the triangles PQR, PRS and PSQ are equilateral. Thus the primitive cell, taken individually, does not feature all the symmetry elements of the face-centered cubic lattice (in particular the 4-fold axes). This is the reason for choosing the quadruple face-centered cubic cell. Thus, for three-dimensional lattices, several multiple cells are used to describe lattices featuring more symmetry elements than the primitive cell shows. Each multiple cell deﬁnes a lattice mode. If the cell that describes the lattice is a primitive cell, the lattice mode is said to be primitive, and it is noted as P. If the cell is base-centered (double cell), the lattice mode is A or B or C depending on whether the centered bases are respectively the faces (b, c) or (c, a) or (a, b). The generic designation for this type of centering is S (for side-face centered). If the cell is body-centered (double cell), the lattice mode is I (as in “inside”), and if the cell has all of its faces centered (quadruple cell), it is noted F (as in “face”). The reader will easily check that these multiple cells do deﬁne a crystal lattice. In contrast, a cell to which one would attempt to add

Chapter 3 – Crystal lattices

51

2c* P’ R’ c

P

A* B*

S

A b

Q B C

Q’

S’

2b*

2a*

R

C*

a

(b)

(a)

Figure 3.15: Face-centered cubic lattice (a) and its reciprocal lattice (b) nodes at the centers of four pair-wise parallel faces does not deﬁne a crystal lattice (Exercise 3.6). To each crystal system there correspond one or several lattice modes. The set of all these lattice modes form the 14 Bravais lattices, distributed over the 7 crystal systems. The rule for determining which Bravais lattice, hence which unit cell, should describe a given structure is to choose the cell (a) featuring the symmetry of the lattice and (b) with the smallest volume. Two examples are very illuminating: the face-centered cubic lattice quoted above, and the body-centered cubic lattice, for which the primitive cell is a rhombohedron with angle α = 109.47◦ (cos α = − 1/3) (Fig. 3.16).

A

B

C

Figure 3.16: The body-centered cubic lattice. The primitive cell is deﬁned by the vectors A, B and C.

52

Symmetry and Physical Properties of Crystals

One may ask why all of the lattice modes are not deﬁned in each of the crystal systems. Actually, some multiple (centered) cells provide no improvement over the primitive cell or over some other multiple cell with lower multiplicity, or again the multiple cell does not feature the symmetry of the lattice any more. Consider for example the tetragonal lattice. There is no advantage in deﬁning a tetragonal lattice in which the square base (a, b) is centered, since the unit cell built on the half-diagonals of the square, a and b , and the vector c is tetragonal too (Fig. 3.17). Furthermore, it can be shown that a face-centered tetragonal unit cell can be described by a centered cell twice as small (Exercise 3.10). A tetragonal unit cell with two opposite non-square faces centered is not a tetragonal cell, since the lattice built on this cell does not have a 4-fold axis any more. The only multiple tetragonal unit cell is the tetragonal body-centered cell, for which no primitive cell can represent the tetragonal symmetry of the lattice.

c

b’

b

a’

a

Figure 3.17: A tetragonal lattice with its square base centered does not need to be considered. The primitive cell, with basis vectors a , b and c, is tetragonal.

3.7.2. The fourteen Bravais lattices The last column of Table 3.3 indicates for each crystal system the various lattice modes. There are all together 14 Bravais lattices (1 triclinic, 2 monoclinic, 4 orthorhombic, 2 tetragonal, 1 rhombohedral, 1 hexagonal, and 3 cubic). Two rows were set aside for the monoclinic system, in order to be able to state the denomination of the base-centered lattices. In this case, the bases which can be centered are the rectangular faces parallel to the 2-fold axis. If we choose to call c the basis vector parallel to this axis, then the lattice mode can be A or Btype. If we choose to call it b, then it can be C or A-type. The orthorhombic lattice modes can be primitive (P), body-centered (I), face-centered (F), or base-centered A, B or C (generically, side-face centered, i.e. S), since the three faces can be centered. The triclinic, rhombohedral and hexagonal lattices can only be primitive. The rhombohedral lattice mode is usually noted R rather than P. The reason will be given in Chapters 5 (Sect. 5.6) and 6 (Sect. 6.3.3). The tetragonal lattice modes can be primitive (P) or centered (I), and the cubic lattice modes can be primitive (P), body-centered (I) or face-centered (F).

Chapter 3 – Crystal lattices

53

It can be shown that an F tetragonal lattice mode can be described via an I lattice mode (Exercise 3.10) and an F or I monoclinic lattice mode via an A or C lattice mode (Exercise 3.11), in full agreement with their absence among the Bravais lattice modes.

3.7.3. Reciprocal lattices of the non-primitive lattices We take as an example the face-centered cubic lattice, and search for its reciprocal lattice, the latter being deﬁned by starting from a primitive cell of the direct lattice. Let a, b, c be the basis vectors of the multiple (quadruple) cubic unit cell, and A, B and C the basis vectors of a primitive cell (Fig. 3.15a) such that A=

1 (b + c), 2

1 B = (c + a), 2

1 C = (a + b). 2

Let us denote the volume of this primitive cell by v0 , and let us determine the basis vectors A∗ , B∗ , C∗ of the reciprocal lattice, starting with A∗ . 1 1 (B × C) = [(c + a) × (a + b)] v0 4v0 1 [(c × a) + (c × b) + (a × b)]. = 4v0

A∗ =

(3.16)

Let a∗ , b∗ , c∗ be the basis vectors of the lattice reciprocal to the direct lattice for which the primitive cell would be the cube built on a, b and c. The volume (a, b, c) of this cubic unit cell of the direct lattice is 4v0 , so that 1 (b × c), 4v0 1 b∗ = (c × a), 4v0 1 (a × b). c∗ = 4v0 a∗ =

Equation (3.16) thus yields A∗ = b∗ − a∗ + c∗ . Similarly, we obtain B∗ = c∗ − b∗ + a∗ , C∗ = a∗ − c∗ + b∗ . If we build the reciprocal lattice starting from this primitive cell (A∗ , B∗ , C∗ ), we see that the lattice is body-centered cubic, the edges of the cube being the vectors 2a∗ , 2b∗ , 2c∗ (Fig. 3.15b). Note: the volume V ∗ of this body-centered cubic reciprocal unit cell is 8 times the volume v ∗ of the unit cell built on a∗ , b∗ and c∗ . Since v0 is the volume of

54

Symmetry and Physical Properties of Crystals

the primitive cell (the rhombohedron with angle 60◦ ), the volume of the unit cell built on a, b, c is 4v0 and the volume of its reciprocal cell (see Sect. 3.2.3) is v ∗ = 1/(4v0 ). We thus obtain V ∗ = 8v ∗ = 2/v0 . Since this reciprocal cell is body-centered, the volume of the primitive reciprocal unit cell is half this volume, i.e. 1/v0 as expected. The above derivation, which showed that the reciprocal lattice of a facecentered cubic lattice is a body-centered cubic lattice, was made on the basis of vector relations, without using the fact that the unit cell is cubic. The same derivation would apply for the orthorhombic face-centered lattice, and this would yield a body-centered reciprocal orthorhombic lattice. The orthorhombic reciprocal cell would have basis vectors 2a∗ , 2b∗ , 2c∗ if we again call the basis vectors of the direct orthorhombic cell a, b and c and those of the corresponding reciprocal lattice a∗ , b∗ and c∗ . The same approach shows (Exercise 3.13) that the reciprocal lattice of a bodycentered cubic lattice with basis vectors a, b and c is a face-centered cubic lattice with basis vectors 2a∗ , 2b∗ and 2c∗ . In the same way (Exercise 3.14), the reciprocal lattice of a base-centered lattice is shown to be a base-centered lattice.

3.8. Surface crystal lattice This section is related to a special area of crystallography: the study of surfaces. It is mandatory for whoever has any interest in investigating crystal surfaces. This research area developed considerably over the last years due to the importance of two-dimensional surfaces and interfaces in many phenomena such as catalysis, corrosion, the manufacturing of metal-semiconductor junctions, etc. To understand the mechanisms involved in these processes, the ﬁrst step consists in investigating plane surfaces with well-deﬁned crystal orientation and with low Miller indices, in order to determine their structure. The atoms located near the surface lose, due to the cut, some of their bonds. They must rearrange, together with their neighbors, in order to ﬁnd a new equilibrium position. This rearrangement can extend over several atomic layers near the surface. One then deﬁnes on the one hand the “bulk” of the crystal, with its three-dimensional periodic structure, and on the other hand the “surface”, which usually consists of several atomic layers, displaced with respect to their position in the bulk, and possibly with a diﬀerent stoichiometry. We also note that the study of surfaces is related not only to clean crystal surfaces, but also to the way foreign atoms, called adatoms, deposit on the surface. The “surface”, thus deﬁned as the set of atomic layers that are modiﬁed by the cut and possibly by the deposited adatoms, retains a two-dimensional periodicity. It is thus possible to deﬁne a surface crystal lattice. Determining this lattice is the ﬁrst step in an investigation of surfaces.

Chapter 3 – Crystal lattices

55

3.8.1. Cut surface Imagine we cut a crystal parallel to a given plane (hkl), and suppose the cut does not alter the atom positions. We can then determine a surface unit cell, deﬁned as the section of the crystal lattice in the bulk by a plane (hkl). This surface unit cell depends on the surface orientation. Consider the example of a primitive cubic lattice, with basis vectors a, b and c. For an (001) surface, the surface cell is square and has basis vectors a1 = a and b1 = b, while a (101) surface produces a rectangular surface cell with basis vectors a1 = a − c and b1 = b (Fig. 3.18a). Now consider a (101) surface in a body-centered lattice, then in a face-centered lattice. The surface unit cells are diﬀerent. If the bulk lattice is body-centered, the (101) surface unit cell is centered rectangular with basis vectors a1 = a − c and b1 = b (Fig. 3.18b). In the case of the face-centered bulk unit cell, the surface unit cell is simple rectangular, with basis vectors a1 = 1/2(a − c) and b1 = b (Fig. 3.18c). We thus determine easily a surface unit cell called the bulk-derived surface unit cell. We call a1 and b1 the basis vectors of this bulk-derived surface unit cell.

c

c

c b

b

a

b1

b

a

b1 a1

b1 a1

(a)

a

a1

(b)

(c)

Figure 3.18: Bulk-derived (101) surface unit cells in the (a) primitive cubic, (b) body-centered cubic and (c) face-centered cubic lattices

3.8.2. Real surface The existence of the surface alters the atom positions in the surface layer. If the displacements aﬀect only the direction perpendicular to the surface without altering the stoichiometry, the bulk-derived unit cell is retained at the surface. This case is referred to as relaxation of the atomic positions. However, surface atoms usually rearrange, thus altering the lattice unit cell at the surface. The surface is said to reconstruct. A simple case of rearrangement or reconstruction is that of the (101) surface of gold. Gold has in the bulk a face-centered cubic lattice. The crystal motif consists of one atom only, so

56

Symmetry and Physical Properties of Crystals

that Figure 3.18c can represent the atom positions in a unit cell. Figure 3.19a shows the atom positions which would prevail on the (101) surface if there were no reconstruction. The full circles correspond to the atoms in the ﬁrst layer, and the empty circles to the second layer. It so happens that the surface reconstructs so that the atoms of every other row parallel to the [10¯1] row in the ﬁrst layer disappear (Fig. 3.19b). This is described by saying that there is a missing row. The reconstructed surface unit cell, i.e. the unit cell of the real surface, then has as its basis vectors a2 = a1 = 1/2(a – c) and b2 = 2b1 = 2b. b2

b1 − [101]

a1

a2

(a)

(b)

Figure 3.19: Reconstruction of the (101) surface of gold. The full circles represent the positions of atoms in the ﬁrst layer, the empty circles those of the second layer and the gray ones those of the third layer. The upper part of each ﬁgure shows a top view; the lower part shows a cross-section. (a) The state of the surface if no reconstruction occurred. (b) Reconstructed surface, with its missing row parallel to [10¯1].

3.8.3. Notations The basis vectors (a2 , b2 ) of the real surface unit cell are generally expressed as a function of the basis vectors (a1 , b1 ) of the bulk-derived unit cell through the relations:

or

a2 = m11 a1 + m12 b1 , b2 = m21 a1 + m22 b1

a1 a2 =M . b2 b1

Matrix M deﬁnes the surface lattice completely. In the case of the (101) surface of gold which we just discussed, M is especially simple:

1 0 . 0 2 Another notation, due to Elizabeth A. Wood, is frequently used although it is not as general since it applies only to cases where: 1.

The angle between vectors a2 and b2 is the same as that between a1 and b1 .

Chapter 3 – Crystal lattices 2.

57

The lengths of a2 and b2 are expressed as a function of those of a1 and b1 by relations: a2 = p a1 and b2 = q b1 .

Noting ϕ the angle by which the surface lattice possibly has turned with respect to the bulk-derived lattice, the lattice for the (hkl) surface of a material with formula Y is indicated as: Y (hkl)(p × q)Rϕ. The simple case of the (101) surface of gold is thus described as Au (101) (1 × 2). We note that the rotation part is omitted if the lattice did not turn. In this notation, the bulk-derived cell is often designated as the (1×1) unit cell. Two examples of surface reconstructions where Wood’s notation can be used are shown on Figures 3.20 and 3.21. Figure 3.20 shows the reconstruction of a (001) surface of tungsten (W), cooled to below room temperature. This crystal is body-centered cubic with edge a, and the motif contains only one W atom. Figure 3.20a shows the atoms of this surface, as seen from above, if there were no reconstruction. The atoms in the ﬁrst layer are the empty circles, and those of the second layer are gray circles. The bulk-derived surface cell is a square with edges a and b, so that a1 = a and b1 = b. Due to the reconstruction, the ﬁrst layer atoms undergo a displacement along the arrows, thus creating, in a [1¯10] direction, a zigzag-like pattern, where the angle is no more 90◦ (Fig. 3.20b). The surface unit cell is a square (full lines on Fig. 3.20b), √ rotated by 45◦ with respect the bulk-derived cell, and its edge is a 2. It √ to √ is described as W (001) ( 2 × 2) R45◦ . It is sometimes described using the square face-centered cell (dotted lines) which is not rotated with respect to the bulk-derived cell, and it is then noted as c(2×2) with c standing for “centered”. b1 = b

a1 = a

(a)

(b)

Figure 3.20: Reconstruction of the W (001) surface. The empty circles represent the atoms of the ﬁrst layer, the gray circles those of the 2nd layer. (a) Bulk-derived cell. The arrows indicate the displacements which the atoms undergo during reconstruction. (b) Reconstructed surface and its primitive (full lines) and centered (dotted lines) unit cells. The second example deals with a surface covered with adatoms, the (111) surface of silicon (face-centered cubic lattice), covered with 1/3 of a monolayer of silver. The bulk-derived unit cell of a (111) surface of a fcc lattice is a hexagonal unit cell with basis vectors a1 = 1/2 [10¯1] and b1 = 1/2 [¯110]

58

Symmetry and Physical Properties of Crystals

represented on Figure 3.21a, where the atoms in the ﬁrst layer are full circles and those of the second layer are empty circles. The Ag atoms deposit above every third atom of the second layer, forming a regular lattice (large circles in thick lines in Fig. 3.21b). The surface unit cell is hexagonal, √ turned by 30◦ with respect to the bulk-derived cell, and the edge length is 3 times larger than the √ edge√of the bulk-derived hexagonal unit cell. It is described as Ag/Si (111) ( 3 × 3) R30◦ .

b1

a1 b2

(a)

a2

(b)

Figure 3.21: Reconstruction of a (111) surface of silicon covered with a third of a monolayer of silver. (a) Clean bulk-derived unit cell. The full circles represent the ﬁrst-layer atoms and the empty circles the secondlayer atoms. (b) Surface covered with Ag atoms, represented by large thick-line circles and located above second-layer atoms.

3.8.4. Reciprocal lattice Interpreting (X-ray or electron) diﬀraction by surfaces involves deﬁning a surface reciprocal lattice. It is therefore necessary to associate to the basis vectors of the surface unit cell a vector which is not in the surface plane. The appropriate vector is the smallest vector of the bulk crystal lattice perpendicular to the surface, and it is noted as n. a2 and b2 being the basis vectors of the unit cell of an (hkl) surface, the reciprocal lattice of the unit cell (a2 , b2 , n) is then deﬁned by the vectors a∗2 , b∗2 , n∗ such that a∗2 = b∗2 = n∗ =

b2 × n , V n × a2 , V a2 × b2 . V

V , the volume built on vectors a2 , b2 and n, is such that V = n · (a2 × b2 ). We note that the vector n∗ is perpendicular to the surface and its norm is equal to the reciprocal of the norm of vector n. For the reconstructed surfaces discussed above, the relevant vectors n are: 1 surface Au (101) (1 √ × 2)√: n = /◦2 [101], surface W (001) ( 2 √ × 2)√R45 : n = [001], surface Ag/Si (111) ( 3 × 3) R30◦ : n = [111].

Chapter 3 – Crystal lattices

59

3.9. Exercises Exercise 3.1 1.

Determine the indices (hkl) of the plane that goes through the three nodes (1, 0, 0), (0, 1, 0) and (0, 0, 3).

2.

Show that the three rows [211], [120] and [302] are coplanar. What are the indices of their common plane?

3.

Determine the row common to the planes (311) and (1¯10).

Exercise 3.2 Titanium oxide TiO2 has a tetragonal lattice with parameters a = 4.59 Å and c = 2.96 Å. 1.

What is the angle between faces (101) and (10¯1)?

2.

Show that, in this system, row [hk0] is perpendicular to plane (hk0), but that the same does not apply to row [0kl] and plane (0kl).

3.

Calculate the lattice distance of planes (321).

Exercise 3.3 1.

Consider a plane crystallographic lattice with basis vectors a and b. We choose an axis system Oxy parallel to a and b, with unit lengths a and b respectively. Consider the row D that goes through points M and N, with coordinates respectively (2, 0) and (0, 3). Determine: (a) the equation of row D. (b) the number of rows parallel to D located between D and the origin O of the lattice. (c) the equations of the rows belonging to this family that go through the point with coordinates (1, 0) and (0, 1) respectively.

2.

Consider the three-dimensional crystallographic lattice with basis vectors a, b as given in (1) and c, where c is a general lattice vector which does not belong to plane (a, b). (a) Determine the values of h, k and l for the family (hkl) of lattice planes parallel to vector MN and c. (b) Determine the values of h, k and l for the family (hkl) of lattice planes parallel to the plane that goes through MN and through the point P with crystallographic coordinates (0, 0, 1).

60

Symmetry and Physical Properties of Crystals

Exercise 3.4 Hexagonal lattice: we recall that the basis vectors a, b and c of the unit cell are such that a = b = c and that the angles are α = β = 90◦ and γ = 120◦ . 1.

Determine the reciprocal lattice of the hexagonal lattice, and give its orientation with respect to the direct lattice.

2.

Calculate the length of the vector [110]∗ of the reciprocal lattice. Deduce the value of the lattice distance between (110) planes. Retrieve this result through a geometrical argument without using the reciprocal lattice.

3.

Calculate the angle between planes (120) and (100).

Exercise 3.5 Consider a hexagonal lattice. The plane (hkil) closest to the origin of the lattice intersects plane (a, b) along a line which intersects vector a at point M such that OM = a/h, vector b at point N such that ON = b/k and vector d at point Q such that OQ = d/i. Vector d is deduced from b through a rotation by 120◦ around c. Draw a ﬁgure in plane (a, b) and note that a + b + d = 0. 1.

Express the area of triangles OMN, OMQ and OQN as a function of the cross product of two of the basis vectors a, b or d.

2.

By writing that the area of OMN is the sum of the areas of OMQ and OQN and by substituting for d its value as a function of a and b, show that you obtain the relation h + k + i = 0.

3.

Consider the (1 2 3 1) lattice plane family. Determine the lattice plane family which deduces from it through a rotation by 2π/3, then the family obtained through a rotation by 4π/3. In the same way, determine the families of planes obtained through symmetry with respect to plane (a, c) and with respect to plane (b, c) respectively.

Exercise 3.6 Show that the set of points consisting of the nodes of a crystal lattice and the points at the centers of four pairwise parallel faces of the unit cell, do not form a crystal lattice. In other words, a crystal lattice cannot have two distinct faces that are centered. Note that crystal periodicity implies that every face deduced through a lattice translation from one that is centered must also be centered. Exercise 3.7 Consider the crystal structures, with cubic lattice, shown on Figures 8.3 (CsCl, NaCl, ZnS) and 8.6 (diamond). Determine their Bravais lattice and their motif. Same question for the structures of Figure 8.4: cubic CaF2 , tetragonal TiO2 and cubic CaTiO3 .

Chapter 3 – Crystal lattices

61

Exercise 3.8 Consider the structure of graphite shown on Figure 8.11. 1.

Draw a projection onto the plane of the hexagons, indicating their heights, of the atom positions. Take as a unit twice the distance between two neighboring carbon planes.

2.

Determine the unit cell, its parameters using the data shown on Figure 8.11, and the number of atoms per unit cell.

Exercise 3.9 The structure of a compound consisting of nickel and gadolinium can be represented as follows. Decompose space into a set of identical right prisms, with regular hexagons as their bases, and contacting one another. Each apex and each center of the lateral faces of the prism is occupied by a nickel atom. The Gd atoms are located at the centers of the hexagonal bases of the prism. In the basal plane, the shortest Ni–Gd distance is 2.83 Å and the height of the prisms is 3.97 Å. 1.

Determine the chemical formula of this compound.

2.

Draw a projection of the atom positions onto the basal plane, stating the heights, and deduce the lattice and the motif.

3.

With the lattice now deﬁned, give the Miller indices of the prism faces.

4.

Calculate the angle between planes (1¯10) and (110).

Exercise 3.10 Show that a tetragonal F (face-centered) lattice mode can be described by a tetragonal body-centered unit cell (I type lattice mode) with half the volume. It will be useful to make a projection of the lattice nodes onto a plane perpendicular to the basis vector c, mentioning the heights. Exercise 3.11 Show that a monoclinic F lattice mode can be described by a monoclinic I lattice mode with a unit cell half the volume, and that this I lattice mode can be described by a base-centered monoclinic unit cell with the same volume. It will be useful to draw a projection of the lattice nodes onto the plane normal to the 2-fold axis of the initial monoclinic lattice, specifying the heights. Exercise 3.12 Draw a projection onto the plane (111) of the nodes of a cubic F lattice, indicating the heights. Show that this yields a ﬁgure similar to Figure 3.14c. Use the fact that direction [111], parallel to a major diagonal of the cube, is a 3-fold axis for the (111) planes which are perpendicular to it.

62

Symmetry and Physical Properties of Crystals

Exercise 3.13 Consider a body-centered cubic lattice with basis vectors a, b and c. Let A, B and C be the basis vectors of the primitive rhombohedral unit cell: 1 A = (b + c − a), 2

1 B = (c + a − b), 2

1 C = (a + b − c). 2

Call a∗ , b∗ and c∗ the basis vectors of the reciprocal unit cell of a primitive cubic unit cell with basis vectors a, b and c. 1.

Determine the basis vectors A∗ , B∗ and C∗ of the reciprocal lattice as a function of A, B and C, then as a function of a∗ , b∗ and c∗ .

2.

Show that the reciprocal lattice of the body-centered cubic unit cell with basis vectors A∗ , B∗ and C∗ is a face-centered cubic lattice with basis vectors 2a∗ , 2b∗ and 2c∗ .

Exercise 3.14 Consider any base-centered lattice, for example A-type, with basis vectors a, b and c. Choose as basis vectors of the primitive unit cell the vectors A = a,

1 B = (b − c), 2

1 C = (b + c). 2

Let a∗ , b∗ and c∗ be the basis vectors of the reciprocal unit cell of a primitive lattice, with basis vectors a, b and c. Show that the reciprocal lattice of the A-type base-centered lattice is a basecentered A-type lattice with basis vectors a∗ , 2b∗ and 2c∗ .

Chapter 3 – Crystal lattices

63

Appendix 3A. The metric tensor The metric tensor is particularly useful for numerical calculations.

3A.1. Deﬁnition The term tensor will be explicitly deﬁned and discussed in Chapter 9, but the formal deﬁnition is not needed here. The term metric means it deals with measure, here the lengths and angles between the basis vectors of the crystal unit cell. The components of the metric tensor are deﬁned by the dot products of the basis vectors of the unit cell, which we note as a1 , a2 and a3 , i.e. the ai with i ranging from 1 to 3, so that gij = ai · aj . The metric tensor is also deﬁned in reciprocal space: ∗ gij = a∗i · a∗j .

3A.2. Volume of the unit cell The volume V of the direct unit cell is: V = a1 · (a2 × a3 ) = (a1 , a2 , a3 ). We express the basis vectors of the unit cell in an orthonormal basis {e1 , e2 , e3 }: a1 =

3

B1j ej

j=1

which can be written using Einstein’s convention, deﬁned in Section 9.3.1. Einstein’s convention consists in suppressing the summation sign (which becomes implicit) in a product of factors when the subscript over which the summation is to be performed is repeated. Thus we can write a1 = B1j ej . Since the subscript j appears twice, it is clear that summation must be performed over j. In a similar way, we write for each of the basis vectors ai : ai = Bij ej . It is easy to check that (a1 , a2 , a3 ) = det B (e1 , e2 , e3 ) where det B is the determinant of the matrix {Bij } or B matrix.

64

Symmetry and Physical Properties of Crystals

Since the basis {e1 , e2 , e3 } is orthonormal, its volume is equal to 1, hence V = det B,

(3A.1)

gij = ai · aj = Bik ek · Bjl el = Bik Bjl ek · el = Bik Bjl δkl = Bik Bjk .

(3A.2)

T where B T is the transposed matrix of B. Bjk can be substituted by Bkj T , so that g = BB T if we call g the matrix {g }, and We obtain gij = Bik Bkj ij

det g = det B det B T = (det B)2

(3A.3)

since the determinants of a matrix and of its transpose are equal. Comparing (3A.1) and (3A.3), we see that V 2 = det g.

(3A.4)

It is on the basis of this formula that, in Section 3A.5 below, the volume of the triclinic unit cell will be easily calculated.

3A.3. Product of the matrices associated to the direct and reciprocal metric tensors ∗ = a∗ · a∗ , where The reciprocal metric tensor is deﬁned by the coeﬃcients gij i j ∗ the ai (i = 1 to 3) are the basis vectors of the reciprocal unit cell.

Let us express the vectors a∗i in the direct basis {a1 , a2 , a3 }: a∗i = Mik ak and

∗ gij

=

a∗i

·

a∗j

= Mik ak · a∗j = Mik δkj = Mij

since the reciprocal lattice vectors are deﬁned by relations (3.4), which can be written: a∗i · ak = δik where δik is Kronecker’s symbol, equal to 1 if i = k and equal to 0 otherwise. Using ∗ a∗i · ak = Mij aj · ak = Mij gjk = gij gjk ,

we obtain ∗ gjk = δik . gij

This relation shows that the product of the matrices g and g∗ is equal to the unit matrix E gg ∗ = E.

(3A.5)

Chapter 3 – Crystal lattices

65

The calculation of the reciprocal metric tensor is therefore performed by inverting the matrix associated to the direct metric tensor. Taking the determinant of both sides of Equation (3A.5), we obtain: det g det g∗ = 1. It can be shown that det g∗ = (V ∗ )2 , as was done for the volume of the direct unit cell, and we retrieve the fact that the volume of the reciprocal unit cell is equal to the reciprocal of the volume of the direct unit cell.

3A.4. Calculation of lattice distances The lattice distance of a family of planes (hkl) is given by relation (3.8): dhkl =

1 1

=

hi a∗ . h∗ i

∗ and We can write hi a∗i 2 = (hi a∗i ) · (hj a∗j ) = hi hj gij

dhkl =

1 ∗ hi hj gij

(3A.6)

which is easily calculated knowing the reciprocal metric tensor which is calculated by inverting matrix g (Eq. (3A.5)).

3A.5. Applications The metric tensor can be written, with the usual notations for the parameters of the crystal lattice: ⎞ ⎛ ab cos γ ac cos β a2 bc cos α ⎠ . b2 g = ⎝ ab cos γ ac cos β bc cos α c2 The determinant of this matrix is given by det g = a2 b2 c2 (1 − cos2 α − cos2 β − cos2 γ + 2 cos α cos β cos γ) whence we deduce through (3A.4) the volume V of the unit cell: V = abc 1 − cos2 α − cos2 β − cos2 γ + 2 cos α cos β cos γ. Inverting matrix g leads to matrix g∗ , so that ⎛ 2 2 2 ⎞ b c sin α abc2 Kαβγ ab2 cKγαβ 1 g∗ = 2 ⎝ abc2 Kαβγ a2 c2 sin2 β a2 bcKβγα ⎠ V ab2 cKγαβ a2 bcKβγα a2 b2 sin2 γ where we use the temporary notation cos α cos β−cos γ = Kαβγ , with two other coeﬃcients Kβγα and Kγαβ being obtained through a circular permutation of the subscripts.

66

Symmetry and Physical Properties of Crystals

Since g∗ is a symmetrical matrix, the general expression (3A.6) of dhkl is given by dhkl =

1 ∗ h2 + g ∗ k 2 + g ∗ l2 + 2g ∗ hk + 2g ∗ hl + 2g ∗ kl g11 22 33 12 13 23

and, in the most general case of the triclinic unit cell, we obtain: 1 − cos2 α − cos2 β − cos2 γ + 2 cos α cos β cos γ dhkl = A with h2 k2 l2 hk sin2 α + 2 sin2 β + 2 sin2 γ + 2 (cos α cos β − cos γ) 2 a b c ab hl kl + 2 (cos α cos γ − cos β) + 2 (cos β cos γ − cos α) ac bc

A=

Chapter 4

Relationship between space groups and point groups After showing that the symmetry operations of a crystal form a group, we show how to go over from this group to the space group characterizing the crystal structure on the microscopic scale, and then to the point group, which governs its macroscopic physical properties. The rigorous proof is preceded by an example which allows the reader to grasp these notions intuitively.

4.1. Introduction The most general symmetry operation which any object, and in particular a crystal, can have can be noted [S(O), t] where S represents a rotation or a rotoinversion (deﬁned in Sect. 2.1) whose axis goes through point O, and t a translation. In the case of rotoinversion, O is also the associated symmetry center. Note that point O, which deﬁnes the position of the axis, has no reason not to change from one operation to another. We will show in the next section that the symmetry operations [S(O), t] of the crystal make up a group. Among all these symmetry operations, there is the set of lattice translations T, and it is interesting to consider the symmetry operations [S(O), t] modulo the lattice translations. The expression “[S(O), t] modulo the lattice translations” means that we do not distinguish operations [S(O), t] and [S(O), t+n] if n is any lattice vector (n belonging to T). It will be shown that these operations form a group, called the position group or space group of the crystal. Consider the direction of a straight line in the crystal, parallel to a vector D, and submit it to any one of these symmetry operations. It becomes another straight line, parallel to vector D such that D = [S(O), t] D = S(O) D = S D

(4.1)

because D is unaltered by any translation t. Reference to point O was suppressed because the result D does not depend on the position of the rotation axis, nor on the point on the axis which is used for inversion when the operation

© Springer Science+Business Media Dordrecht 2014 C. Malgrange et al., Symmetry and Physical Properties of Crystals, DOI 10.1007/978-94-017-8993-6_4

67

68

Symmetry and Physical Properties of Crystals

is a rotoinversion. The only relevant data are the direction of the axis and the rotation angle. Since D is deduced from D through a symmetry operation of the crystal, the macroscopic properties measured along directions D and D will be the same (for example, the elongation of a bar parallel to D or to D under the inﬂuence of a given increase in temperature). We thus understand that the symmetry of the macroscopic properties of the crystal is governed by the operations S solely deﬁned by the direction of a rotation (or rotoinversion) axis and the rotation (or rotoinversion) angle. We will show in Section 4.3 that these operations S comprise a group, called the orientation group of the crystal or the point group. The latter term reminds us that, for this group, all the symmetry elements can be made to go through a given point, since the position of the symmetry element does not matter. The point group is thus obtained from the space group of the crystal by ignoring all translations (or, equivalently, by replacing all translations with the zero translation), and by having all the rotation or rotoinversion axes go through one given point, which will also be the center of symmetry used if there is a rotoinversion. In order to illustrate the notions of space group and point group, consider the plane periodic ﬁgures of Figure 4.1, which we assume to extend to inﬁnity. They can be considered as sorts of two-dimensional crystals. Figure 4.1a (the crystal lattice of which is shown in Fig. 4.1b) features two families consisting of an inﬁnity each of mirrors, parallel to one another and perpendicular to the plane of the ﬁgure. The mirrors of one of the families are denoted as Mi and the symmetry operation associated to mirror Mi is designated as mi (symmetry with respect to plane Mi ). The mirrors of the other family, perpendicular to the mirrors Mi , are denoted as Mj and the associated symmetry operations as mj . The symmetry operations of this plane crystal have the form [mi , ua+vb] and [mi , u a+v b],1 where u, v, u and v are integers and a and b are the basis vectors of the lattice. We must add to these operations the products of these operations. These product operations are rotations by 180◦ , denoted Rk , around axes perpendicular to the plane lattice, located at the intersections of the mirrors, followed by lattice translations, hence [Rk , u a + v b]. We will show (Exercise 4.1 and Sect. 7.2.2) that the product of a mirror operation m (symmetry with respect to a mirror plane M) by a translation t perpendicular to the mirror is a pure mirror operation where the new mirror is deduced from M by a translation t/2. We thus obtain: [m1 , b] = [m2 , 0];

[m1 , 2b] = [m3 , 0];

[m1 , −b] = [m0 , 0];

etc.

(4.2)

¯ axis normal to the mirror 1. Here we simpliﬁed the notation. A mirror is equivalent to a 2 for which the reference symmetry center is located at the point where the axis intersects the mirror. The notation consistent with [S(O), t] would, for operation (mi , ua +vb) (see Sect. 4.2.1), be [¯ 2(Oi ), ua + vb], with point Oi located at the intersection of the ¯ 2 axis with the plane Mi .

Chapter 4 – Relationship between space groups and point groups

69

M’0 M’1 M’2 M3 M2 M1 M0

b

M–1

a

(b)

(a) M’1

O’ a/2

O

M1 b a

(c)

(d)

Figure 4.1: Examples of plane “crystals” (a) and (c) and their crystal lattices (b) and (d) The mirror operations [m1 , vb] with v an integer thus describe the set of operations [mi , 0]. The set of operations [mi , ua+vb] can thus be replaced by the set [m1 , ua+vb] where m1 is the operation associated to any one particular mirror chosen as the reference (here M1 ), and u and v any integers. This set of symmetry operations, modulo the lattice translations T, can be represented by operation [m1 , 0]. The same reasoning applied to operations [mj , u a + v b] modulo T shows that [m1 , 0] can represent the set of operations [mj , u a + v b] modulo T and that [R1 , 0] can represent the set of operations [Rk , u a + v b] modulo T. The symmetry operations of this crystal, modulo the lattice translations T, are thus identity, a mirror operation m1 , a mirror operation m1 , and operation R1 , a rotation by π around the intersection of the mirrors M1 and M1 . This is a set Gs such that: Gs = [E, 0] + [m1 , 0] + [m1 , 0] + [R1 , 0] modulo T. These symmetry operations make up the space group. The point group G0 , obtained by deleting all translations and having all the symmetry elements go through the same point, is thus: G0 = [E, 0] + [m1 , 0] + [m1 , 0] + [R1 , 0]. Now consider the “crystal” of Figure 4.1c, whose lattice, shown on Figure 4.1d, is identical to that of Figure 4.1a. It also features two families of mirrors, but the mirrors of family Mi are glide mirrors (Sect. 2.2.4), the symmetry operation of which is the product of operation mirror mi and of translation a/2.

70

Symmetry and Physical Properties of Crystals

The symmetry operations of this crystal have the form [m1 , (u + 12 )a + vb], [m1 , u a + v b] and their products. The mirror operations of the space group are now [m1 , a/2] and [m1 , 0] modulo the lattice translations. The space group is thus: Gs = [E, 0] + [m1 , a/2] + [m1 , 0] + [R , 0] modulo T. Operation R is a rotation by 180◦ around the axis intersecting the plane of the ﬁgure at point O deduced from O, the intersection of the traces of M1 and M1 , through translation a/4 (Exercise 4.2). The point group G0 is obtained from Gs by suppressing all translations and having all the symmetry elements go through one single point. We obtain: G0 = [E, 0] + [m1 , 0] + [m1 , 0] + [R1 , 0]. The two “crystals” we are discussing have diﬀerent space groups but the same point group G0 . Further in this chapter, we will show rigorously how to go over from the group of symmetry operations which the crystal features, to its space group, and from the space group to the point group. This will require the use of the quotient group notion. It is deﬁned in Appendix 4A, a refresher on some properties of groups which may be useful reading. However, the reader may be content, on a ﬁrst quick reading, with the approach just given. It provides a feeling for the point group and space group notions and their relationship. The reader can then go over directly to the next chapter, Chapter 5, which lists in a logical way the various point groups which crystals can feature.

4.2. Symmetry operations of the crystal 4.2.1. Change in origin A symmetry operation [S(O), t] transforms point M1 into point M2 such that OM2 = S(OM1 ) + t. Let us show that we can change origin, i.e. ﬁnd S , O and t such that [S (O ), t ] = [S(O), t]. O M2 = S (O M1 ) + t

Then

(4.3)

for any M1 . Let us explicit both sides of Equation (4.3). O M2 = O O + OM2 = O O + S(OM1 ) + t.

(4.4)

S (O M1 ) + t = S (O O + OM1 ) + t = S (O O) + S (OM1 ) + t .

(4.5)

Chapter 4 – Relationship between space groups and point groups

71

Since the right hand sides of Equations (4.4) and (4.5) are equal, we deduce that S(OM1 ) + t = S (OM1 ) + S (O O) − O O + t which must be true for any point M1 . This implies that: S = S,

(4.6)

t = t + (S − E)(OO )

(4.7)

where E is the identity operation. We can therefore replace all the symmetry operations [S(O), t] featured by the crystal with operations [S(O ), t ] where O is now common to all the symmetry operations, provided each translation t is replaced by translation t given by Equation (4.7). We can thus choose a reference point common to all the symmetry operations, hence simplify the notation by not mentioning this reference point. This will be done throughout the remainder of this chapter. We denote as (S, t) the symmetry operations featured by a crystal, with the understanding that a point O common to all the symmetry operations of the crystal has been chosen. We now show that these operations form a group, the symmetry group of the crystal.

4.2.2. The operations (S, t) form a group The product of two symmetry operations of a crystal is of course also a symmetry operation. Let us look for the expression of the product of two of these operations, viz. (S1 , t1 ) which changes M into M1 and (S2 , t2 ) which transforms M1 into M2 . OM1 = S1 (OM) + t1 OM2 = S2 (OM1 ) + t2 = S2 S1 (OM) + S2 t1 + t2 whence

(S2 , t2 )(S1 , t1 ) = (S2 S1 , S2 t1 + t2 ).

(4.8)

Search for the neutral element: by using relation (4.8), we easily check that the neutral element is (E, 0) where E is the identity operation. The proof is (E, 0)(S, t) = (S, t)(E, 0) = (S, t). Search for the inverse element: we want to determine (S, t)−1 = (S , t ) such that (S , t )(S, t) = (E, 0). From (4.8), (S , t )(S, t) = (S S, S t + t ) hence S S = E and S t + t = 0. Therefore

S = S−1 , t = −S−1 t.

(4.9)

72

Symmetry and Physical Properties of Crystals

S−1 is the inverse operation of S. Consider an example: if S is a rotation by 2π/3 around a given axis (which goes through the point O common to all the symmetry operations), S−1 is a rotation by −2π/3 around the same axis. The translation t is the opposite of the vector deduced from t through a rotation by −2π/3 around the axis (Fig. 4.2). M’

M1

t

S −1(t)

M

O

t’ = −S −1(t) M’1

Figure 4.2: Illustrating the inverse operation of (S, t), where S is the rotation by 2π/3 around an axis perpendicular to the plane of the ﬁgure and going through O. M1 is the transform of M under this operation. The rotation by −2π/3 around the same axis transforms M1 into M1 , and translation t = − S−1 t brings M1 back to M.

4.2.3. The lattice translations form an invariant subgroup of the group of symmetry operations of the crystal To prove this result and that of the next section, we use a few deﬁnitions and properties of invariant subgroups and of quotient groups given in Appendix 4A. The lattice translations are the symmetry operations (E, n) where E is the identity operation and n = ua + vb + wc, a, b and c are the basis vectors of the unit cell and u, v, w are integers. We show that the set of operations (E, n) form a group, which is a subgroup of the symmetry operations (S, t) of the crystal. The product of two lattice translations is a lattice translation, and the neutral element (E, 0) is part of this set. Let us show that this subgroup is invariant (Appendix 4A), i.e. that, for any S, we have: (S, t)(E, n)(S, t)−1 = (E, n ). (S, t)(E, n)(S, t)−1 = (S, t)(E, n)(S−1 , −S−1 t) = (S, t)(S−1 , −S−1 t + n) = (E, −SS−1 t + Sn + t) = (E, Sn). (E, Sn) is a pure translation. It is a symmetry operation of the crystal since it was obtained as the product of symmetry operations of the crystal. Since its rotation part is identity, it is necessarily a crystal lattice translation.

Chapter 4 – Relationship between space groups and point groups

73

Conclusion 1.

The set of lattice translations is an invariant subgroup of the group of the symmetry operations of the crystal.

2.

We showed that Sn is a crystal lattice vector. This result shows that the operations S are symmetry operations of the lattice. We will see at the end of Section 4.3 that the reciprocal proposition is not necessarily true.

4.3. Space groups and point groups The subgroup (E, n) = T of the lattice translations being invariant, we can deﬁne a quotient group G/T starting from the partition of G by T (Appendix 4A). The partition of G into cosets products of T by symmetry operations of the crystal which are not lattice translations can be expressed as G = T + T(S1 , t1 ) + T(S2 , t2 ) + T(S3 , t3 ) + . . . + T(Sm , tm ). This partition is performed in the following way: we isolate within G a ﬁrst packet of operations, here the lattice translations T. Among the remaining operations, we choose an operation (S1 , t1 ). We perform the product of this operation by all the lattice translations, forming the second packet T(S1 , t1 ), and so forth until all the elements of G have been used. We here operate with the smallest possible vectors (null or smaller than a lattice vector) by subtracting from the initial translation vector tj as large a lattice vector ni as possible. This lattice vector ni may then be included in T. This is possible since (Si , tj ) = (Si , ti + ni ) = (E, ni )(Si , ti ) so that

T(Si , tj ) = T(Si , ti ).

We will determine further (Sect. 7.2) the symmetry operations (Si , ti ), where ti is a non-zero vector smaller than a crystal lattice vector, which may exist in a crystal. We will see that they are the symmetry operations associated to screw axes or to glide mirrors (Sect. 7.2.1 and 7.2.2). The quotient group is deﬁned as Gs = G/T, the group whose elements are the cosets T(Si , ti ). If we consider the symmetry operations modulo T, we can replace coset T(Si , ti ) by (Si , ti ). We can then write Gs = (E, 0) + (S1 , t1 ) + (S2 , t2 ) + (S3 , t3 ) + . . . + (Sm , tm ) modulo2 T. In the introduction to this chapter, we deﬁned two operations equivalent modulo T as two operations for which the diﬀerence in the translation parts 2. Adding “modulo T” is mandatory in order for the above operations to form a group because it can happen that the product of two of the operations (Si , ti ) is equal to (Sj , tj + n) while, as mentioned above, the ti are smaller than lattice translations.

74

Symmetry and Physical Properties of Crystals

is equal to a lattice translation n. (E, n)(S, t) = (S, t + n).

This is indeed the case here since

Gs is called the space group, or position group, of the crystal. Now consider the operations (E, 0), (S1 , 0), (S2 , 0), etc. which deduce from the elements of Gs by canceling all the translations, i.e. by canceling the “modulo T” and replacing the ti by 0. Using the composition law (4.8), it is easy to show that these operations form a group G0 , isomorphous to Gs , which can be written G0 = (E, 0) + (S1 , 0) + (S2 , 0) + (S3 , 0) + . . . + (Sm , 0). This group is the point group (or orientation group) of the crystal. It is obtained by considering all the symmetry operations of the crystal, deﬁned, as we remember, with a common origin (Sect. 4.2.1), and by canceling all translations. We saw, at the end of Section 4.2.3, that the operations (Si , 0) are symmetry operations of the lattice. The reciprocal proposition is not necessarily true (and indeed it is often wrong), i.e. all symmetry operations of the lattice are not necessarily symmetry operations of the point group. We note that: The symmetry operations of the point group of the crystal form a subgroup of the symmetry operations of the crystal lattice. A simple example, chosen from among the plane lattices, is given on Figure 4.3a. The crystal features a family of pure plane mirrors Mi , and does not feature any mirror perpendicular to the Mi . The point group of the crystal is G0 = (E, 0) + (m, 0) where m is the symmetry operation associated to one of the mirrors Mi . M3 M2 M1 M0

b

M–1

(a)

Figure 4.3: lattice in (b)

a

(b)

(a) An example of a plane “crystal”, with its crystal

The crystal lattice (Fig. 4.3b), for which the unit cell is a rectangle, features a family of mirrors Mi perpendicular to the Mi . Let us denote with m the symmetry operation associated to one of the mirrors Mi , and with A the product of operations m and m , i.e. the rotation by π around their intersection. The point group of the crystal lattice is G0 = (E, 0) + (m, 0) + (m , 0) + (A, 0)

Chapter 4 – Relationship between space groups and point groups

75

and indeed G0 is a subgroup of G0 . As was discussed at the beginning of this chapter, the point group of the crystal is very important because it governs the symmetry of the macroscopic properties of crystals. Furthermore, the construction of space groups is easy to explain when starting from the point groups. We therefore start by investigating the point groups or orientation groups (Chap. 5) and then, in Chapter 7, we show how the space groups or position groups can be built starting from the point groups. For a given point group, it is useful to know the directions that are equivalent to a given direction through the symmetry operations which are elements of the group. These equivalent directions are represented using the stereographic projection, deﬁned in the next chapter.

4.4. Exercises Exercise 4.1 Show that the product of a symmetry with respect to a plane P and a translation by a vector V perpendicular to plane P is a symmetry with respect to the plane P deduced from P by a translation V/2. Consider a general point M, its image M1 by symmetry with respect to P, and then the point M2 , image of M1 through translation V. Draw the ﬁgure in the plane Π perpendicular to P and going through M. Exercise 4.2 1.

Show that the product of a symmetry with respect to a plane P1 and a symmetry with respect to a plane P2 perpendicular to P1 is a rotation by π around zz , the intersection of planes P1 and P2 .

2.

Now replace the second symmetry operation of (1) by the operation product of the symmetry with respect to P2 and a translation V perpendicular to zz and parallel to plane P2 . Show that this ﬁnal operation is a rotation by π around an axis deduced from zz through a translation V/2.

76

Symmetry and Physical Properties of Crystals

Complement 4C. Probes used for crystal structure determination 4C.1. Possible probes and criteria for choice Crystal structure research mainly involves the determination of the nature of the atoms comprising the material and their arrangement in space. This process is invariably based on coherent scattering, i.e. diﬀraction. It therefore requires probes that interact with atoms, with a wavelength smaller than the distances between atoms, viz. 1 Å = 1 ×10−10 m = 0.1 nm. The wavelength is given by λ = h/p where h is Planck’s constant h = 6.63 ×10−34 J s and p the probe momentum. There are three possibilities: X-rays, neutrons and electrons. Electrons can be eﬀectively focused through magnetic lenses, giving the possibility of either imaging or diﬀraction modes in the electron microscope. Neutrons and X-rays can be focused, either by reﬂection from curved mirrors or crystals, or through diﬀractive lenses (zone plates, or Fresnel lenses), or through the use of refractive lenses consisting of stacks of small spheres or paraboloids, or holes in materials. Much better results are obtained in the case of spatially coherent beams of synchrotron X-rays3 . These three probes interact with diﬀerent features of matter. X-rays interact with the electrons within materials, stronger scattering being associated with atoms with more electrons, i.e. with heavier atoms. Neutrons are sensitive to the nature of the nuclei (number of protons, i.e. chemical nature, but also number of neutrons, hence isotope) and also to the magnetic ﬁelds within matter. Electrons sense the electrostatic potential due to both the nuclei and the electrons. In structural work, the fact that there is no systematic relation between the strength of nuclear scattering (the nuclear scattering length) of thermal neutrons and the atomic number of the scatterer opens up possibilities for elegant approaches complementary to X-ray diﬀraction. Electrons are strongly absorbed by materials, and can go through thin samples only (typically less than 1 micrometer), while X-rays, and even more neutrons, can go through thick samples. These probes are also very diﬀerent in their ease of production and in the intensity of the beams that can be obtained. The probe with by far the widest use is X-rays.

4C.2. X-rays X-rays are electromagnetic waves. They have the proper range of wavelength λ, around 1 Å, when their photon energy E = hc/λ where c is the velocity of light in vacuum, is of the order of 10 keV. They are produced, like all electromagnetic waves, when light electric charges (in eﬀect electrons) are accelerated. The standard sources for X-rays are laboratory X-ray tubes, in which electrons are accelerated by a voltage V on the order of 104 V and hit a metal target, the anode. X-rays are emitted both in the form of “character3. Christian David, http://www.psi.ch/lmn/x-ray-optics

Chapter 4 – Relationship between space groups and point groups

77

istic” radiation, i.e. fairly ﬁne spectral lines, and in the form of a continuous spectrum, Bremsstrahlung.4 The characteristic lines correspond to transitions of atomic electrons between discrete atomic energy levels as the electron vacancies induced by the incoming electrons heal, and their energies or wavelengths depend on the target material. X-rays are also produced, with much higher intensity than in laboratory X-ray tubes, as part of the synchrotron radiation emitted when the trajectories of ultra-relativistic electrons or positrons (energy E much larger than their rest mass energy me c2 = 0.511 MeV) are curved by a magnetic ﬁeld. Synchrotron radiation covers a huge spectral range, from the infrared, through the visible and ultra-violet range, to high-energy X-rays if the energy of the electrons or positrons is high enough, and it is the hard X-ray part (typically 10 to 100 keV energy, or about 0.1 to 0.01 nm wavelength) that is put to use for structural work. Monochromatic beams (beams with a given energy or wavelength) must be prepared through monochromators. In practice, synchrotron radiation sources are storage rings into which the particles are fed after being accelerated to energies of several GeV. Initially considered by high energy physicists as a nuisance, synchrotron radiation is now the sole motivation for the construction of “dedicated” machines. Beyond intensity, synchrotron radiation oﬀers, among the features useful in structure determination, the possibility of tuning the wavelength, and in particular of aiming for selected values where the response of one given type of atoms is enhanced by resonance. For most structure investigations, laboratory X-rays, obtained from X-ray generators which are aﬀordable for normal size laboratories, are satisfactory; access is then easy for the researchers. In some special cases, higher intensity or other requirements make it desirable to use hard X-rays from synchrotron radiation sources. These large facilities, with high construction and operation cost, are mostly available in developed countries. For example, in 2011, APS (Advanced Photon Source) in the USA, Spring8 in Japan and ESRF in Europe, Diamond the British source, Petra III the new German source, Swiss Light Source (SLS), Soleil the French one, all are third-generation, i.e. highest-performance sources. They are accessible to researchers on the basis of applications for beam-time which are ranked by committees, a procedure which takes time – and does not always lead to acceptance. Thus their use is eﬀectively reserved for work, much of which is outside structural crystallography, which cannot be performed with laboratory X-rays. Novel large facilities for the production of X-rays are appearing: free electron lasers or XFEL (X-ray Free Electron Lasers). They produce pulses of coherent X-rays with extremely large intensity and a duration of less than 100 femtoseconds. This makes it possible to envisage watching atomic movements in solids, understanding chemical reac4. Bremsstrahlung (with a capital B ) is the German word for “radiation from braking”. It is associated with the decrease in velocity of electrons through interaction with the target material. Energy conservation immediately yields a useful feature: the energy of a photon cannot be more than that of the electrons, thus the short-wavelength limit of the spectrum is such that hc/λmin = eV .

78

Symmetry and Physical Properties of Crystals

tion processes on the molecular scale, etc. Two such sources are operational in 2011: LCLS (Linac Coherent Light Source) at Stanford, CA, USA since 2009, while SACLA (Spring-8 Angstrom Compact free electron Laser) in Harima, Japan produced its ﬁrst beams in 2011. Others are being built: the European source XFEL in Hamburg, Germany and SwissFEL in Villigen, Switzerland, PAL (Pohang Accelerator Laboratory) in Korea.

4C.3. Neutrons Neutrons are particles with rest mass mn = 1.67 ×10−27 kg, with no electric charge but with a magnetic moment μn = −0.97 ×10−26 J T−1 with the minus sign indicating that the magnetic moment is in the direction opposite to the spin. Neutron beams are produced either from nuclear reactors, using ﬁssion, or from spallation sources in which high energy proton beams interact with a target, usually in a pulsed mode5 . Examples of research reactors are the multinational Institut Laue-Langevin (ILL), and Orphée at the Laboratoire Léon Brillouin in Saclay, near Paris. ISIS, in England, or the Spallation Neutron Source (SNS) in Oak Ridge, TN, USA, are spallation sources. In either case, the initial energy of the neutrons, in the MeV range, is much too high for structural investigations, and they have to be submitted to a decrease in their kinetic energy, a process called moderation. They have De Broglie wavelength in the right range, around 1 Å, if their kinetic energy Ec = p2 /2mn = h2 /2mn λ2 , where p is their momentum, is a few tens of meV. A diﬀerent way of expressing this condition is that the kinetic energy then corresponds to a thermal energy kB T where kB = 1.38 ×10−34 J K−1 is Boltzmann’s constant and T a temperature in the range around room temperature, i.e. 300 K. This description is meaningful because preparing neutron beams in the right range of energy is actually performed by letting the neutrons, which cannot be tailored by electric ﬁelds, collide with a moderator material, such as heavy water D2 O, at this temperature. They are usually called “thermal neutrons”, while neutrons with higher energy, obtained through moderation in a hot object, are “hot neutrons”, and those with lower energy are “cold” or “ultra-cold” neutrons. As in the case of synchrotron radiation, single-energy beams must be extracted through the use of monochromators. The intensity of neutron beams is smaller than that of X-ray beams from laboratory generators, and very much smaller than X-ray beams from synchrotron radiation. Furthermore, neutrons are only available at large facilities, which implies the same diﬃculties in access as for synchrotron radiations. This leads to their use being far less wide-spread than X-rays, and restricted to investigations where their special features are a bonus.

5. Recommended reading includes two courses by Roger Pynn: http://www.ncnr.nist.gov/summerschool/ss09/pdf/Lecture_1_Theory.pdf, and http://link.springer.com/book/10.1007/978-0-387-09416-8/page/1.

Chapter 4 – Relationship between space groups and point groups

79

4C.4. Electrons Electrons are particles with electric charge −e = −1.6 ×10−19 C, with rest mass me = 0.9 ×10−30 kg. Their magnetic moment, associated to the intrinsic angular momentum or spin, has a direction opposite to the spin. Its absolute value is 1 Bohr magneton (1μB ) = 0.93 ×10−23 J T−1 , much larger than the neutron’s but whose inﬂuence is hidden by the eﬀect of the charge. The relation between the kinetic energy eU , obtained through acceleration under voltage U , and the De Broglie wavelength of an electron6 is: λ= √

1 h . 2m0 eU 1 + eU 2 2m0 c

Electrons with wavelength in the range of 10−10 m are unable to penetrate materials, and they can provide information from a very thin region near the surface (Low Energy Electron Diﬀraction, LEED). Higher energy electrons (100 keV or more) are used for the investigation of thin ﬁlms (less than 1 micrometer) in electron microscopes. These allow switching between the imaging and diﬀraction modes, i.e. between the observation of direct and reciprocal space, at the press of a button. They are complementary to X-rays for some crystal structure investigations, in particular for materials where only tiny crystalline regions can be obtained.

Further reading J. Als-Nielsen, D. McMorrow, Elements of Modern X-ray Physics, 2nd edn. (Wiley, 2011) R. Scherm, B. Fåk, Neutrons, in Neutron and Synchrotron Radiation for Condensed Matter Studies, vol. 1: Theory, Instruments and Methods, ed. by J. Baruchel et al. (Les Editions de Physique and Springer-Verlag, 1993) R. Pynn, Introduction to Neutron Scattering. A clear and comprehensive exposition is available on http://knocknick.ﬁles.wordpress.com/2008/04/neutronsa-primer-by-rogen-pynn.pdf. The “rogen” in the address is a misprint for “roger”; in case it gets corrected at some point, the revised address could be tried in case of diﬃculty.

6. The general expression for the De Broglie wavelength of a particle is the relativis tic expression λ = h/p = hc/pc, with pc = E 2 − m20 c4 . It is well introduced in http://hyperphysics.phy-astr.gsu.edu/hbase/quantum/debrog2.html#c2. The limiting cases for zero rest mass (ultrarelativistic case, e.g. photons) and for kinetic energy small with respect to the rest mass energy (non-relativistic case, e.g. thermal neutrons) are easily retrieved.

80

Symmetry and Physical Properties of Crystals

Appendix 4A. General features of groups Deﬁnition A group is a set G of elements g1 , g2 . . . featuring an internal composition law, here denoted as •, so that f = gi • gk , and f is an element of G. This composition law is associative: gi • (gk • gl ) = (gi • gk ) • gl , so that the parentheses can be omitted in this product has a neutral element e such that gi • e = e • gi = gi is such that each element gi has an inverse g−1 such that gi • g−1 = i i −1 gi • gi = e. In what follows, we will omit the sign •. Order of the group If G is an inﬁnite set of elements, we say that the group is inﬁnite. Otherwise, we say that it is ﬁnite, and the order of the group is the number of its elements. Generating elements These are elements of the group such that all the elements of the group can be obtained as products of powers of these elements with one another or with their inverses. Rearrangement theorem The multiplication table of group is a dual-entry table (Sect. 2.3). All elements of the group appear on each row and each column of the table, and no element appears twice on a given row or column. This means that if x = y, then xz = yz. Proof: if xz = yz, then xzz −1 = yzz −1 and x = y, which is contrary to the assumption. Note that each row or column of the multiplication table contains all the elements of the group, but ordered diﬀerently from the preceding row or column. This is why this is referred as rearrangement theorem. Subgroup A subgroup H is a part of the elements of group G that forms a group with the same composition law as group G itself. We will show that, if group G is ﬁnite, the order nG of G is a multiple of the order, nH , of H. The ratio i = nG /nH is called the subgroup index. Invariant subgroup A subgroup H (with elements denoted as hi ) of G is invariant if, for any element s of G and hi of H, we have s−1 hi s = hj or hi s = shj .

Chapter 4 – Relationship between space groups and point groups

81

Partition of a group G modulo a subgroup H This is a classiﬁcation of elements of group G. We start out by considering the elements of H and withdrawing them from G. Then there remains in G at least one element x. We form all the products xhi . This set is denoted as xH and we remove it. We show that xH is disjoint from H. Assume in contrast that xhi = hj . Right-multiplying both sides of this equation by h−1 i , we obtain , which is an element of H since H is a group. But this is contrary x = hj h−1 i to the starting assumption (x is not in H). If there still remains in G an element y, we form the subset yH, we withdraw it from what remains of G, and so forth till there is nothing left. We can write G = H + xH + yH + . . . We show that xH and yH are disjoint by noting that, if we had yhi = xhj , then y = xhj h−1 i = xhk and this is contrary to the assumption (y is not in xH). Each subset xH or yH is called a coset. Since each coset of this partition has the same number of elements as H, we deduce that, if H and G are ﬁnite, the order of G is a multiple of the order of H. The above partition was performed by left-multiplying the elements of H with x, y, etc. It could have been made by choosing right-multiplication. Both partitions have no reason to be identical. In contrast, they are identical if H is invariant, because then xhi = hj x and in this case the set xH is identical to the set Hx. Quotient group Consider the partition of G by an invariant subgroup H. We show that the cosets xH, yH, etc. form a group which is called the quotient group of G by H and is denoted by G/H. The product of two elements xH and yH of this group is deﬁned as the set of elements obtained through the product of one of the elements of xH by one of the elements yH, i.e. xhi (yhk ) = x(hi y)hk = x(yhp )hk

because of the associativity in G, since H is invariant,

= xy(hp hk ) through associativity in G, = xyhm

because H is a group.

We deduce that the product of xH by yH is xyH, i.e. (xH)(yH) = (xy)H. The product xy cannot be within H since x and y are outside H, and thus xy = z with z ∈ / H and z = x or y; otherwise x or y would be the neutral element of G which is also the neutral element of H, and thus within H. Thus (xH)(yH) = zH. Associativity is obvious since associativity applies within G. The neutral element is H, since hi (y hn ) = hi (hp y) = (hi hp )y = hv y = yhw and thus H(yH) = yH. The inverse of xH is x−1 H since xhi x−1 hn = xx−1 hp hn = hq .

82

Symmetry and Physical Properties of Crystals

Abstract groups A group can be deﬁned by the name of its elements and their multiplication table without reference to concrete examples. It is then referred to as an abstract group. Here are two examples: 1.

Cyclic groups They are groups denoted as Cn which have n elements such that, if one is denoted as A, the others are A2 , A3 ,. . . ,An = E where E is the neutral element. For example, group C3 consists of an element A, of element A2 and of the neutral element E = A3 . Its multiplication table is given below A

A2

E

A

A2

E

A

A2

E

A

A2

E

A

A2

E

As we will see, a concrete realization of this group is the group of rotations by 2π/3 around an axis, i.e. in terms of point groups, group 3. 2.

Dihedral groups A dihedral group is deﬁned using two generating elements A and B which satisfy relations B2 = E, An = E and BA = An−1 B. It includes 2n elements and is denoted as Dn . We will see that a concrete realization of group D3 is for example point group 32, for which A is the rotation by 2π/3 about a given axis and B is the rotation by π around an axis perpendicular to the above.

Chapter 5

Point groups The point groups are enumerated in a rigorous way. On ﬁrst reading, the reader can be content with their geometrical representation using the stereographic projection (Sect. 5.2) and with their denomination and classiﬁcation by crystal system (Sect. 5.6).

5.1. Introduction The point group of a crystal governs the symmetry of its physical properties. We recall that the point group consists of the symmetry operations of the crystal with all the translations removed. All the symmetry elements are assumed to go through a given point O. Further, we saw (Sect. 2.1) that the symmetry elements which do not contain a translation are either rotations or rotoinversions. The rotations are operations which conserve the handedness of a trihedron (proper operations), while the rotoinversions, which do not conserve the handedness of a trihedron, are said to be improper operations. We showed (Sect. 4.3) that the symmetry operations of the point group form a subset of the point group of its crystal lattice. This property also results from Curie’s principle (Sect. 3.3.5) because the crystal lattice is a property of the crystal and therefore it must be at least as symmetric as the crystal. This is a basic result, because it restricts the number of proper crystallographic point groups (groups which contain only proper operations, i.e. rotations). Since the only symmetry axes which a crystal lattice can feature are the 2-, 3-, 4- or 6-fold axes, the proper symmetry operations of crystals are the symmetry operations associated to 2-, 3-, 4- or 6-fold axes. We will ﬁrst enumerate the proper crystallographic point groups (Sect. 5.4), after showing that the improper groups always contain a proper subgroup with order half their own (Sect. 5.3). This property will be used in Section 5.5 to enumerate the improper groups starting from the proper groups. Sections 5.3, 5.4 and 5.5 show how to logically enumerate the 32 crystallographic point groups. In a ﬁrst approach, the reader may accept that there are 32 point groups, and get acquainted with them straight away in Section 5.6, where they are grouped into crystal systems. In contrast, reading

© Springer Science+Business Media Dordrecht 2014 C. Malgrange et al., Symmetry and Physical Properties of Crystals, DOI 10.1007/978-94-017-8993-6_5

83

84

Symmetry and Physical Properties of Crystals

Section 5.2, which introduces the stereographic projection used to represent the point groups, is mandatory. The chapter closes with a short discussion of isotropy groups in Section 5.9. They are not crystal point groups, but they enter the investigation of the physical properties of crystalline materials.

5.2. Stereographic projection 5.2.1. Deﬁnition It is very useful to represent, for a given point group, the directions equivalent to a given general direction, i.e. the directions obtained from this direction by applying all the symmetry operations which make up this group. For a general direction, i.e. a direction which is not parallel to a symmetry axis (n-fold or n ¯ -fold axis), there is one direction for each symmetry operation, and therefore there are as many equivalent directions as there are symmetry operations in the group. A precise two-dimensional representation of these equivalent directions requires a projection of three-dimensional space onto the plane of the drawing. The projection used by crystallographers is the stereographic projection, deﬁned below. Let O be the intersection of the various symmetry elements (rotation or rotoinversion axes).1 A given general direction is represented by a half-line Ov starting from this point O. This half-line intersects a sphere with center O and with any radius R at a point P which characterizes the direction (Fig. 5.1a). Representing the half-lines is tantamount to projecting the points P of the sphere onto a plane. We choose a projection plane Π which goes through the center of the sphere. This plane Π intersects the sphere along a circle C. We draw the diameter NS perpendicular to plane Π; N is the north pole, S the south pole, Π is the equatorial plane and circle C the equatorial circle. Let Ov be a direction in the northern hemisphere. Consider the meridian plane deﬁned by axis NS and point P (Fig. 5.1b). The line SP of this plane intersects the equatorial projection plane Π at n, which is the required projection. The triangles NPS and nOS are similar, and SN/Sn = SP/SO. We obtain Sn . SP = SN . SO = 2R2 . Point n is therefore deduced from P through an inversion with pole S and power 2R2 . Recall the deﬁnition of the inversion transformation. An inversion with pole O and power k transforms a general point M into an image point M such that O, M and M are aligned and OM . OM = k. Inversion conserves angles and transforms a circle that does not go through pole O into a circle.

1. For rotoinversion axes, this is also the position of the center of symmetry used for the rotoinversion operations.

Chapter 5 – Point groups N

N

v

v P

P

A

O

A

n

C

85

O

B

B

x

n

n'

P' v'

S

S

(a)

(b)

N A A

O

m

B

n'

O

n 9

m B

P' v' S

(c)

x

(d)

Figure 5.1: Principle of the stereographic projection. (a) The general direction Ov intersects the sphere at P. (b) n and n are respectively the transforms of P and P in inversions with pole S, the south pole. (c) m is the transform of P through inversion with pole N, the north pole. (d) n and m are the stereographic projections of the directions Ov and Ov respectively. Point P is deﬁned by its spherical coordinates R, θ and ϕ (axis Ox is a general direction in plane Π), and its projection n by its polar coordinates ρ and ϕ in plane Π. The length ρ = On is easily calculated when we notice that (SP, SN) = α = θ/2. Hence On = R tan α = R tan(θ/2). It is important to note that the azimuthal coordinate ϕ is conserved by the stereographic projection. Now consider a direction Ov in the southern hemisphere, and, in order not to clutter the text with more ﬁgures than necessary, assume it is in the same meridian plane as the above direction Ov (Fig. 5.1b). It intersects the sphere at P . Its projection n , deﬁned as above, is outside the equatorial disk. The closer P comes to the south pole, the further n moves away from O. This would lead, in order to represent all the directions of space, to using an inﬁnite surface! To avoid this diﬃculty, we use, for the directions of the southern hemisphere, an inversion with pole N, and with the same power 2R2 (Fig. 5.1c). The projection m of direction Ov is now located inside the equatorial disk. The stereographic projection is thus deﬁned as an inversion with pole S (the south pole) for the directions located in the northern hemisphere, and an inversion with pole N (the north pole) for the directions in the southern hemisphere. Thus the same

86

Symmetry and Physical Properties of Crystals

point will be the projection of two directions, symmetric to each other with respect to the projection plane Π. To distinguish these projections, one uses two diﬀerent symbols, for example crosses for the projections of the directions in the northern hemisphere, and circles for those of the southern hemisphere (Fig. 5.1d). The equatorial disk thus contains the stereographic projections of all the directions of space.

5.2.2. Examples Consider the point group 3, i.e. the group whose elements are the rotations by 2π/3, 4π/3 and 2π (identity) around a given 3-fold axis denoted as A3 . We choose as projection plane for the equivalent directions a plane perpendicular to this axis A3 . The projection of the axis itself is point O, the common projection of the directions ON and OS. Consider a general direction Ov, the stereographic projection of which is n, with polar coordinates (ρ = On, ϕ) (Fig. 5.1a). Rotation around axis NS causes rotation of the meridian halfplane containing Ov and conserves angle θ, hence ρ. The projections of the three directions equivalent to Ov through the three symmetry operations of the group are n (ρ, ϕ + 2π/3) for the rotation by 2π/3, n (ρ, ϕ + 4π/3) for the rotation by 4π/3 and n itself for the rotation by 2π or identity (Fig. 5.2). We understand, using this simple example, that the number of directions equivalent to a given general direction is equal to the number of elements in the symmetry group, or order of the group. Of course this is no more true if the direction is special, as would be the direction of the axis itself, which is invariant through the symmetry operations, and the stereographic projection of which is O. n’

O

n

n”

Figure 5.2: Stereographic projection of a general direction (projection at n) and its equivalent directions through the symmetry operations associated to an axis A3 The point symmetry elements featured by a crystal with a given crystal group appear directly on the stereographic projection of the directions equivalent to a general direction through the symmetry operations of the group. In what follows, we will simplify our description by simply referring to the “stereographic projection of the equivalent directions”, the remainder of the sentence being implied. A few examples are illustrated on Figure 5.3. The derivation of the results is either evident, or given in Appendix 5A.1. The thick lines represent the stereographic projections of planes, while the thin lines are just aids for the drawing.

Chapter 5 – Point groups

87 B

O

7

B

O A

A

(a)

B

O

O A

(b)

(c)

(d)

Figure 5.3: Stereographic projections of various symmetry elements and of the directions equivalent through the symmetry operations to which they are associated: (a) mirror in the projection plane; (b) mirror perpendicular to the projection plane; (c) 2-fold axis in the projection plane; (d) general mirror intersecting the projection plane along AB Mirror parallel to the projection plane: it coincides with plane Π. Its stereographic projection is the equatorial circle. Two directions which are equivalent through the mirror operation project on the same point with diﬀerent symbols, since one of the directions is in the northern hemisphere and the other in the southern hemisphere (Fig. 5.3a and Appendix 5A.1.2). Mirror perpendicular to the projection plane: it goes through axis NS and its projection is the line where the mirror intersects the plane of projection, i.e. AB on Figure 5.3b. The equivalent directions are in the same hemisphere and their stereographic projections are two points with the same nature (cross or circle), symmetric with respect to the line representing the projection of the mirror (Appendix 5A.1.3). n-fold axis, noted An or n, perpendicular to the projection plane: the projection of the axis consists in two points coinciding with the center of the equatorial circle. It is represented by a single symbol, characteristic of its order n. The conventional symbols are given in Table 5.1. The equivalent directions, all located in the same hemisphere, project on points which deduce from one another through rotations by 2π/n around the axis, and which are represented by the same sign (Fig. 5.4). Table 5.1: Graphical representation of the symmetry axes Axis type 2

Graphical representation

Axis type _ 1

4

_ 3 _ 4

6

_ 6

3

Graphical representation

88

Symmetry and Physical Properties of Crystals

2

3

4

6

Figure 5.4: Stereographic projections of directions equivalent through the symmetry operations associated to 2-, 3-, 4- and 6-fold axes 2-fold axis parallel to the projection plane: the projection of the axis consists in two points A and B, the intersections of the axis and the equatorial circle (Fig. 5.3c). These points are displayed using the symbol characteristic of the 2-fold axes. The equivalent directions are in diﬀerent hemispheres, and their projections are symmetric with respect to line AB (Appendix 5A.1.4). Mirror with general orientation: such a mirror intersects the projection plane along a line AB. The stereographic projection of the mirror consists of two circular arcs going through A and B and symmetric with respect to AB (Fig. 5.3d and Appendix 5A.2.1).

5.2.3. Application to rotoinversion axes or n ¯ -fold axes The deﬁnition of n ¯ -fold axes was given in Section 2.2.2, but their properties can become clearer using the new tool we now have. Figure 5.5 shows the stereographic projections of equivalent directions for these various rotoinversion axes. The projection plane is perpendicular to the n ¯ axis, and goes through the inversion center used for the rotoinversion.

7 7

7

7

– 1

– 2

– 3

– 4

– 6

Figure 5.5: Stereographic projections of directions equivalent through the symmetry operations associated to ¯1, ¯2, ¯3, ¯4 and ¯6-fold axes We note that: a ¯3-fold axis is equivalent to the set consisting of a 3-fold axis (coinciding with the ¯3-fold axis) and a center of symmetry;

Chapter 5 – Point groups

89

a ¯6-fold axis is equivalent to the set consisting of a 3-fold axis (coinciding with the ¯6-fold axis) and a mirror perpendicular to this axis and going through the inversion center used for the rotoinversion; a ¯4-fold axis has no equivalent. ¯ We retrieve the fact that a 1-fold axis is equivalent to a center of symmetry and a ¯2-fold axis to a mirror perpendicular to the axis and going through the center of symmetry used for the rotoinversion. We can note that the order of the n ¯ groups is equal to n, except for the group ¯3 for which the order is 6.

5.2.4. Family of equivalent directions We saw in Chapter 3 that a crystal row is noted [uvw] if the vector V joining two neighboring nodes on the row can be expressed as: V = ua + vb + wc, where a, b and c are the basis vectors of the crystal unit cell. Since the physical properties of a crystal are identical along two directions equivalent through the symmetry operations of its point group, it is often necessary to consider not only a direction parallel to a row [uvw], but the set of directions equivalent through the symmetry operations of the point group. The set of these equivalent directions is noted < uvw >. In the same way, the set of lattice planes equivalent to a lattice plane (hkl) through the symmetry operations of the point group is noted {hkl}. However, we must note that [uvw] represents a row of nodes and is not oriented. In the same way, (hkl) is a lattice plane and its normal is not oriented. When directions equivalent through the symmetry operations of the point group are considered, it is necessary, for the non-centrosymmetric groups, i.e. those which do not contain inversion, to orient the direction. For example, in a crystal with the cubic point group ¯43m, <111> is diﬀerent from < ¯1¯1¯1 > and, in the same way, {111} is diﬀerent from {¯1¯1¯1} (Exercise 5.6). The name given to {hkl} is a “crystal form”. The reason is that the growth rate of a crystal is the same for all the equivalent (hkl) planes. If the external shape or form of the crystal (its “habit”) features an (hkl) orientation, then the whole set of faces equivalent to (hkl) are encountered, whence the name “crystal form” for {hkl} (assuming of course that special external interactions, which could hamper the growth of some faces, are not present).

5.3. Improper groups 5.3.1. Preliminary remark For a given group, we will note Si its proper symmetry operations (rotations) and Sj its improper symmetry operations (rotoinversions). We recall that the

90

Symmetry and Physical Properties of Crystals

product of two proper operations or of two improper operations is a proper operation, and that the product of a proper operation and an improper operation is an improper operation. By deﬁnition, a proper group contains only proper operations, and an improper group contains one or several improper operations. However an improper group contains at least one proper operation: the neutral element. We can therefore write any group G as the sum of a set of proper elements, among which the neutral element E or identity, and of a set of improper elements which is an empty set when G is a proper group: G = {E, S1 , S2 , . . .} + {S1 , S2 , . . . }.

5.3.2. Properties of improper groups The proper elements of an improper group form an invariant subgroup with order half that of the improper group. 1.

They form a group because the product of two proper elements is a proper element, the neutral element is a proper element and the inverse of a proper element is a proper element.

2.

This subgroup is invariant. This requires showing that, for any element s of the group, s−1 Si s = Sj (Appendix 4A). This is evident if s is a proper element. If s is improper and noted as Sk , its inverse Sj is also improper, and we obtain a proper element for the product Sk Si Sj .

3.

This subgroup is of order half that of the group. We will show that an improper group contains as many proper elements as improper elements.

Let np be the number of proper elements and ni the number of improper elements of the group. Consider a given improper element Sm , and multiply it successively by i)

all the np proper elements: Sm Sk = Sl . We obtain np improper elements, all diﬀerent from one another (see the rearrangement theorem derived in Appendix 4A). Therefore np ≤ ni .

ii) all the ni improper elements: Sm Sk = Sl . We obtain ni diﬀerent proper elements, and ni ≤ np . The conclusions of (i) and (ii) imply that ni = np . We deduce from (1), (2) and (3) that an improper group always contains a proper subgroup with order half its own and invariant.2 2. It can be shown that a subgroup of order half is always invariant. Therefore we could have just shown that the subgroup is of order half.

Chapter 5 – Point groups

91

We now enumerate ﬁrst the proper groups, then the improper groups starting from the proper groups.

5.4. Enumeration of the proper point groups 5.4.1. Preamble We recall that the elements of a proper point group are rotations by 2π/n and their multiples around a given axis, with the condition (Sect. 3.3.2): n = 1, 2, 3, 4, or 6 (condition 1). The simplest groups are those which contain only the symmetry operations resulting from the presence of a single symmetry axis, an n-fold axis, often noted as An . They will be enumerated in Section 5.4.2. We then consider the groups which contain symmetry operations associated with the existence of two axes, An and An , where n and n satisfy condition 1. The combination of two of these operations, i.e. the product of a rotation by 2π/n (or one of its multiples) around axis An and a rotation by 2π/n (or one of its multiples) around axis An must also satisfy condition 1, i.e. be a rotation by 2π/n (or one of its multiples) around an axis, with n also fulﬁlling condition 1. This restriction on n leads to the following results: 1.

For a general value of n, n is equal to 2 and the angle between the two axes is equal to 90◦ . The corresponding groups are described in Section 5.4.3.

2.

For n = 2 or 4, n can also be equal to 3 and the angle ω between the 3-fold axis and the 2- or 4-fold axis is then such that cos2 ω = 1/3, i.e. the angle between a side and a major diagonal of a cube. The corresponding groups (cubic groups) are described in Section 5.4.4.

The approach used to derive these results is the following. Let ω be the angle between axes An and An and O their intersection point (Fig. 5.6). We choose a system of axes Oxyz such that axis Oz be parallel to axis An and axis Ox be perpendicular to the plane deﬁned by An and An . The matrix Sn representing the rotation around axis An is easily expressed in the axis system Oxyz. The matrix Sn representing the rotation around axis An is easily expressed in a system of axes Oxy z where Oz is parallel to An , and it is noted Sn . To obtain the matrix Sn for the rotation around An in the axis system Oxyz, we use the transition matrix R for passage from the referential Oxy z to the referential Oxyz. We know that Sn = R−1 Sn R. The product Sn Sn is a matrix for which the trace must be an integer in order to satisfy the condition n = 1, 2, 3, 4 or 6 (Sect. 3.3.2). The calculation is simple but tedious, and will not be presented here.

92

Symmetry and Physical Properties of Crystals An’ An z z’

O

y’ y

x

Figure 5.6: Systems of orthonormal axes used to obtain the product of a rotation around an axis An and a rotation around another axis An’ . Axis Ox is perpendicular to the plane containing An and An’ .

5.4.2. Groups containing only the symmetry operations associated to an axis An (cyclic groups) Note: for simplicity, the title of this section could be replaced by “groups featuring only an axis An ”, and this is what we will often do in what follows even though this formulation is not very accurate. The elements of the group are the symmetry operations associated to the symmetry element, for example the rotations by π/2, π, 3π/2 and 2π for a group “featuring an A4 axis”. There are ﬁve such groups, corresponding to n = 1, 2, 3, 4 and 6, and they are noted n in the Hermann-Mauguin notation which we use in this book. Group 1: no symmetry operation in this group, which contains only the identity element. Group 2: existence of an axis A2 . The symmetry operations are the rotation by π around this axis and the rotation by 2π, i.e. identity. Group 3: existence of an axis A3 . The symmetry operations are the rotations by 2π/3, 4π/3 and 2π (identity) around the axis. Group 4: existence of an axis A4 . The symmetry operations are the rotations by 2π/4 = π/2, π, 3π/2 and 2π (identity) around the axis. Group 6: existence of an axis A6 . The symmetry operations are the rotations by 2π/6 = π/3, 2π/3, π, 4π/3, 5π/3 around the axis, and identity. Figure 5.4 shows the stereographic projection of the equivalent directions for each of these groups. The projection plane is perpendicular to axis An . The number of equivalent directions, equal to the order of the group (Sect. 5.2.2), is equal to n. The corresponding abstract groups are the cyclic groups Cn (Appendix 4A).

5.4.3. Groups containing the symmetry operations associated to an axis An and to a perpendicular axis A2 , or dihedral groups An elementary geometrical argument shows that, if there exist a symmetry axis An and an axis A2 which is perpendicular to it and intersects it at point O,

Chapter 5 – Point groups

93

then there exist n axes A2 going through O, orthogonal to axis An , and with an angle π/n between them (Exercise 5.1). This can also be shown using the stereographic projection (Exercise 5.2). These groups are called n2 if n is odd (group 32) and n22 if n is even (groups 222, 422, 622). The second “2” in the latter cases may seem redundant. Its presence will be justiﬁed when we describe the space groups. The corresponding abstract groups are the dihedral groups Dn (Appendix 4A). Figure 5.7 shows, for each of these groups, the stereographic projection of the equivalent directions and of the symmetry elements.

222

32

422

622

Figure 5.7: Dihedral point groups. They feature one An axis and n 2-fold axes which are perpendicular to An .

5.4.4. Cubic proper groups These are groups for which the generating elements are the symmetry operations associated to a 2-fold (or 4-fold) axis and a 3-fold axis, with the angle between them equal to that between one side of a cube and a major diagonal of this cube. By working out the product of the various symmetry operations associated to the 2-fold (or 4-fold) axis and the 3-fold axis, it can be shown that there are then three 2-fold (or 4-fold) axes parallel to the three sides of a cube, and four 3-fold axes, parallel to the major diagonals of the cube (Exercise 5.3). The two groups thus deﬁned are called 23 and 432. The notation for the cubic groups consists of two or three symbols. The ﬁrst one concerns the symmetry axes parallel to the sides of the cube, the second one the 3-fold axes parallel to the major diagonals of the cube, and the third, if it exists, indicates the presence of axes parallel to the diagonals of the cube faces. We will see later that, in the cubic groups featuring mirrors, the same rule applies when considering the directions perpendicular to the mirrors. Thus the notation 23 indicates the presence of 2-fold axes parallel to the sides of a cube and of 3-fold axes parallel to the major diagonals of the cube. There is no third symbol because there are no symmetry axes parallel to the diagonals of the cube faces. The group 432 involves three 4-fold axes parallel to the sides of the cube, four 3-fold axes parallel to the cube diagonals, and six 2-fold axes parallel to the diagonals of the six cube faces. Figure 5.8 shows, for each of these groups, the stereographic projection of the equivalent directions and the symmetry elements.

94

Symmetry and Physical Properties of Crystals

23

432

Figure 5.8: Proper cubic groups

5.5. Enumeration of the improper point groups We saw that any improper group G contains a proper (and invariant) subgroup of order half. Let us note it as Gp . The group G can thus be decomposed into cosets starting from Gp : ¯ p = {S1 , S2 , . . . , Sp } + {AS ¯ 1 , AS ¯ 2 , . . . , AS ¯ p} G = Gp + AG ¯ is any improper element of G. If G contains inversion, a partition into where A ¯ these two cosets is evident since inversion itself can be chosen as the element A. This is discussed in the next section. We will see in Section 5.5.2 how to obtain those improper groups that do not contain inversion.

5.5.1. Improper groups containing inversion These are obtained by considering successively all the proper groups previously deﬁned, and adding to them one generating element, inversion I (and consequently all the elements that are the product of an element of Gp and of inversion): G = {Gp } + I{Gp }. The stereographic projection of the directions equivalent through the symmetry operations of the group is a good tool to determine all the symmetry operations of the groups G thus obtained. The ﬁrst, almost trivial, example, is that of group 1, the only element of which is identity, to which one adds inversion I. The group contains two elements, the neutral element or identity E, and inversion I. It is noted as ¯1, since a ¯1 axis is equivalent to a center of symmetry (Fig. 5.5). Groups deduced from the cyclic groups Consider the proper group 2 and the improper group to which it is associated by adding inversion. We draw the stereographic projection of the equivalent directions onto a plane perpendicular to the 2-fold axis (Fig. 5.9). Consider an initial direction, and suppose it is in the northern hemisphere. Its stereographic

Chapter 5 – Point groups

95

projection is a cross at point 1. The direction equivalent through a rotation by π around the axis has for its stereographic projection a cross at point 2. Let us add a center of symmetry. The projection of the direction equivalent to 1 through inversion is a circle (since it is a direction in the southern hemisphere) at point 3 coinciding with point 2, and that of the direction equivalent to 2 through inversion is a circle at point 4 coinciding with 1. We therefore immediately see there is a mirror perpendicular to the 2-fold axis.

17 37

4

2

Figure 5.9: Point group obtained by adding inversion to group 2 The group we are discussing has 4 elements, corresponding to the four stereographic projections: identity E associated to the projection 1 of the initial direction, rotation by π around the axis, which we note as A, associated with projection 2 (2 is the transform of 1 through A), inversion I associated to 3 (3 is the transform of 1 through I), and the mirror operation m perpendicular to the axis, associated to 4 (4 is the transform of 1 through m = IA). The generating elements of the group are A and I (the fourth element is then m = AI) or A and m (and the fourth element is I = Am). The notation for this group refers to the second choice. It is noted as 2/m, the position of m as the denominator to 2 meaning that the mirror is perpendicular to the 2-fold axis. Figure 5.10 shows the stereographic projections of the improper groups thus determined by adding inversion to the cyclic groups of Figure 5.4, and their denominations. They are noted 2/m, ¯3, 4/m and 6/m. We recall that the existence of a ¯3-fold axis is equivalent to the presence of a 3-fold axis and of a center of symmetry. 7 7 7

7 7

2 — m

7

7

7

– 1

7

7

– 3

4 — m

7

7

6 — m

Figure 5.10: Point groups obtained by adding inversion to groups 1, 2, 3, 4 and 6

96

Symmetry and Physical Properties of Crystals

Groups deduced from the dihedral groups Consider group 222 and the stereographic projection of the 4 directions equivalent through the symmetry operations of the group onto a plane perpendicular to one of the 2-fold axes (Fig. 5.11a). Let us add inversion to these symmetry operations. We obtain, on the stereographic projection, four further directions, the directions opposite to the above (Fig. 5.11b).

7 7

7 7

222

mmm

(a)

(b)

Figure 5.11: Group 222 and group mmm, deduced from 222 by adding inversion This projection reveals three mirrors perpendicular to the 2-fold axes, and mutually perpendicular. The group is noted mmm because the three mutually orthogonal mirrors can be chosen as generating elements. The presence of the 2-fold axes then results from the product of the mirror operations taken pairwise. In the same way, if inversion is added to group 422, we obtain a 4-fold axis, four mirrors going through the 4-fold axis and enclosing an angle of π/4 between each other, and a mirror perpendicular to the 4-fold axis. The generating elements of the group are the 4-fold axis, a mirror going through the axis, and a mirror perpendicular to the axis. Its denomination is 4 ⁄ m mm. As above, the m as the denominator of the fraction indicates that the mirror is perpendicular to the 4-fold axis. The ﬁnal m is redundant, but its presence is justiﬁed when space groups are considered (Chap. 7). Figure 5.12 shows the stereographic projections of the equivalent directions in the improper groups thus determined, and their denominations (¯3m, 4 ⁄ m mm, 6 ⁄ m mm). 77 7 7

7 7 77

– 3m

7

4 —mm m

7

7

7

7 7

7 7 7

7

7

7

6 —mm m

Figure 5.12: Groups obtained by adding inversion to the dihedral groups 32, 422 and 622. The white circles at the centers of the symbols for the 3-, 4- and 6-fold axes indicate the existence of a center of symmetry.

Chapter 5 – Point groups

97

Groups deduced from the proper cubic groups Adding inversion to group 23 gives group m¯3 (Fig. 5.13, to be compared with Fig. 5.8). The ﬁrst sign (m) indicates that there are mirrors perpendicular to the sides of the cube, and the second sign indicates that the axes parallel to the major diagonals are ¯3 axes. There is no third sign because there are no 2-fold axes parallel to the face diagonals, nor mirrors perpendicular to these diagonals. 7 7 7

7 77 77

7

7 7 7

– m3

7 7 7 7 7 7 77 7 7 7 7 7 7 7 77 7 7 7 7 7 7 7

– m3m

Figure 5.13: Groups obtained by adding inversion to the proper cubic groups Adding inversion to group 432 leads to group m¯3m which features all the symmetry elements of a cube. The reader will check that the symmetry elements of a cube all go through the center of the cube and are the following: a center of symmetry, three 4-fold axes parallel to the cube sides and the mirrors perpendicular to them, four 3-fold axes coinciding with the major diagonals of the cube, six 2-fold axes parallel to the face diagonals of the cube, and the six mirrors which are respectively perpendicular to them, called diagonal mirrors. The denomination of the group also states that there are three mirrors perpendicular to the sides of the cube (ﬁrst m), four 3-fold axes parallel to the major diagonals of the cube and an inversion center (¯3), and six mirrors perpendicular to the face diagonals of the cube (m in third position). The 2-fold axes result from the combination of two orthogonal mirrors and lie at their intersection. The 4-fold axes result from the joint presence of mirrors parallel to the cube faces and of diagonal mirrors.

5.5.2. Improper groups which do not feature inversion We saw in Section 5.3.2 that any improper group G contains a proper invariant subgroup with order half. Let us denote it as Gp . Group G can therefore be split into two cosets starting from Gp : ¯ p = {S1 , S2 , . . ., Sp } + {AS ¯ 1 , AS ¯ 2 , . . ., AS ¯ p} G = Gp + AG ¯ is an improper element which we assume not to be inversion. Consider where A ¯ obtained by multiplying A ¯ and inversion I. This the proper element A = IA may look arbitrary, but we will soon see why it is of interest. Let us show, through a reduction toward the absurd, that A is not part of G or, more precisely, of Gp , since A is a proper element. If A belonged to Gp , then its

98

Symmetry and Physical Properties of Crystals

¯ which belongs to G, inverse A−1 would also be in Gp , and its product with A, −1 −1 −1 ¯ ¯ i.e. A A would be part of G. But A A = IA A = I and, by assumption, I is not in G. Therefore A is not an element of Gp . Consider the set G = Gp + AGp = {S1 , S2 , . . ., Sp } + {AS1 , AS2 , . . ., ASp }. The elements ASk do not belong to Gp . To show this, assume ASk is part −1 −1 of Gp . Since S−1 k is in Gp , the product (ASk )Sk = A(Sk Sk ) = A would also be in Gp , which is contrary to the above result. All the ASk are distinct, since if ASk = ASl , then left-multiplying with A−1 would yield Sk = Sl , which is contrary to the assumption. We now show that G and G are isomorphous, with the following correspondence: the elements of Gp correspond with one ¯ p is associated to ASp . Compare the multiplication tables of another, and AS G and G (Fig. 5.14), which we divided into four quadrants. The top left quad¯ k) = ¯ j )(AS rants are identical. So are the bottom right quadrants, since (AS (IASj )(IASk ) = (ASj )(ASk ) because of the commutativity of I with all the elements and because I2 = E. The top right quadrant contains, for G , the ¯ k ) = Sj (IASk ) = ISj (ASk ). products Sj (ASk ) and for G, the products Sj (AS The bottom left quadrants show for G the products (ASj )Sk and for G the ¯ j )Sk = (IASj )Sk = I(ASj )Sk . There is thus a one-to-one correproducts (AS spondence between the products in G and G. S1 S2

Sk

Sp AS1

ASk ASp

S1 S2 Sj

SjSk

Sj(ASk)

Sp AS1 AS2 ASj

S1 S2

Sk

– Sp AS1

– – ASk ASp

S1 S2 Sj

SjSk

ISj(ASk)

IASjSk

ASjASk

– Sp AS1 – AS1 ASjSk

ASjASk

– ASj – ASp

ASp

G’

G

Figure 5.14: Multiplication table of the isomorphous groups G and G The elements of the set G thus form a proper group of order 2p, isomorphous to G. To each group G2p containing a proper subgroup with order half there will correspond an improper group G as searched for. To obtain G starting from G2p and its subgroup Gp , we proceed in the following way: we separate in G2p the subgroup Gp and its complementary subgroup K, consisting of the operations K1 , K2 , . . . , Kp equivalent to the operations ASi : G2p = Gp + {Ki }.

Chapter 5 – Point groups

99

¯ i required to obtain G are the operations (IA)Si = I(ASi ) = The operations AS IKi . The required group G is: G = Gp + {IKj }. We start with the simplest example: that of group 2 (consisting of identity E and of the rotation A by π around the axis, i.e. {E, A}). This has as its subgroup with order half the group 1, which has as its sole element E. G = E+A and G = E+IA = {E, m} where m = IA is the symmetry operation with respect to a plane perpendicular to the 2-fold axis. This 2-fold axis was used as an intermediate device in the reasoning, but it is not a symmetry element of the group we are investigating. The improper group we are searching for has for its symmetry elements a mirror, and this group is denoted as m. In more complicated cases, the deﬁnition of G starting from G is made much easier by using the projection of the directions equivalent through the elements of G2p and of Gp . We take as an example group 422 and its subgroup with order half, 222. Figure 5.15a is the stereographic projection of the directions equivalent through the symmetry operations of group 422 (G2p ). We choose an initial projection direction, and denote it as 1. Figure 5.15b shows the directions equivalent to 1 through the symmetry operations of group 222 (Gp ). Figure 5.15c shows the equivalent directions for the required group G. The additional directions 5 , 6 , 7 , 8 are the reverse of directions 5, 6, 7 and 8, the complementary of directions 1, 2, 3 and 4 in obtaining 422 starting from 222. We see, on the projection of Figure 5.15c, that this group contains a ¯4-fold axis, two 2-fold axes perpendicular to this axis ¯4, and two mirrors parallel to axis ¯4 and enclosing angles of 45◦ to the 2-fold axes. This group is noted as ¯42m.

5 6 4 3

8’ 7’ 1 2

4 3

1 2

8 7

4 3

1 2 6’ 5’

422

222

– 42m

(a)

(b)

(c)

Figure 5.15: Construction of group ¯42m starting from group 422 (a) and its subgroup with order half, 222 (b) Figure 5.16 shows the stereographic projection of the equivalent directions in these various improper groups that do not contain inversion. We note that 1.

Any group 2n (abstract group C2n ) admits group n (abstract group Cn ) as a subgroup with order half (2→1), (4→2), (6→3) and these associations lead to groups m, ¯4 and ¯6 respectively (Fig. 5.16a).

2.

Groups n22 admit groups n as subgroups of order half, with the associations (222 → 2), (32 → 3), (422 → 4), (622 → 6), which lead to the

100

Symmetry and Physical Properties of Crystals

7 7

7

7

– 4

m

– 6

(a)

mm2

3m

4mm

6mm

(b) 7

7

7

7

7

– 42m

7

– 62m

(c)

– 43m

(d)

Figure 5.16: Point groups obtained from: (a) groups (2n) and their subgroups n; (b) groups n22 and their subgroups n; (c) groups 2p22 and their subgroups p22; (d) group 432 and its subgroup 23 groups mm2, 3m, 4mm and 6mm respectively, called pyramidal groups because they have the symmetry of regular pyramids with an n-fold axis and mirrors going through the axis (Fig. 5.16b). 3.

Groups n22 with n even, i.e. n = 2p, also admit the subgroups with half order p22, with the associations (422→222) and (622→32), which lead to groups ¯42m and ¯62m respectively (Fig. 5.16c).

4.

The cubic group 432 admits group 23 as a subgroup with order half, which leads to the group ¯43m (Fig. 5.16d). This is the symmetry group of a regular tetrahedron.

We thus deﬁned the 32 crystallographic point groups, which are 11 proper groups, 11 improper groups containing inversion, 10 improper groups that do not contain inversion.

Chapter 5 – Point groups

101

5.6. Classiﬁcation of the point groups The set of crystals having a given point group form a crystal class. All classes with the same lattice symmetry form a crystal system. Figures 5.17a and b show the classiﬁcation of point groups (hence of crystal classes) by crystal system. This classiﬁcation will be fully justiﬁed in Chapter 6. The qualitative presentation made here is an easy approach, suﬃcient on ﬁrst reading. We saw that there are seven crystal systems, deﬁned on the basis of the symmetry of the crystal lattice. We also saw that the crystal lattice is at least as symmetric as the crystal or, to put it diﬀerently, that the point group of the crystal is a subgroup of the point group of the crystal lattice or the group itself (Sect. 4.3). Simple examples of crystal point groups which are subgroups of the point group of the crystal lattice are the 21 point groups which do not contain inversion, while the point groups of all crystal lattices do contain inversion. We thus consider the seven point groups that have the symmetry of the seven crystal systems. Each of these groups is called a holohedral group. Each holohedral group is taken as the head of a row on which we arrange its respective subgroups. It is placed at the right-hand end of the row. On a given row, the number of elements of each group (the order of the group) grows from left to right, ending with the holohedral point group, the group of the crystal lattice. Figures 5.17 show, for all groups, the stereographic projection of their symmetry elements (Fig. 5.17a) and the directions equivalent to a given starting direction (Fig. 5.17b). The projection plane is perpendicular to the axis with the highest symmetry, except for groups 23 and m¯3, where the projection is performed, as for all cubic groups, on a plane perpendicular to one side of the cube. The starting direction is the same for all groups, so that the subgroups of the groups show up easily. Consider for example the crystals with an orthorhombic lattice. An orthorhombic lattice (unit cell in the shape of a rectangle parallelepiped) has for its symmetry elements 2-fold axes parallel to the sides of the parallelepiped, mirrors perpendicular to these axes, and a center of symmetry. The corresponding point group is group mmm (the third group starting from the left on the third row). The notation indicates the existence of three mutually orthogonal mirrors, the symmetry operations of which are the generating elements of the group. We showed the existence of crystal point groups 222 (three mutually orthogonal 2-fold axes) and mm2 (two mutually orthogonal mirrors, leading to the presence of a 2-fold axis at their intersection), which are subgroups of group mmm. It follows that a crystal with orthorhombic lattice can have for its point group 222, mm2 or mmm.

102

Symmetry and Physical Properties of Crystals

Triclinic

Bravais modes

P _ 1 - Ci P C (A) 2 - C2

222 - D2

m - Cs

mm2 - C2v

2/m - C2h P I F A (B) (C)

mmm - D2h

P I 4 - C4

_ 4 - S4

4/m - C4h

422 - D4

4mm - C4v

_ 42m - D2d 4/mmm - D4v

R P 3 - C3

_ 3 - C3i

6 - C6

_ 6 - C3h

Hexagonal

Rhombohedral (trigonal)

Tetragonal (quadratic)

Orthorhombic

Monoclinic

1 - C1

32 - D3

3m - C3v

_ 3m - D3d

P 622 - D6

6mm - C6v

Cubic

6/m - C6h

_ 62m - D3h 6/mmm - D6h

23 - T

_ m 3 - Th

432 - O

_ 43m - Td

_ m 3m - Oh

Figure 5.17a: The 32 crystallographic point groups arranged by crystal system: stereographic projection of the symmetry elements. The rightmost column indicates the Bravais modes consistent with each of the systems.

P I F

Chapter 5 – Point groups

103

Triclinic

Bravais modes

P

P C (A) 2

222

m

mm2

2/m P I F A (B) (C)

mmm

P I 4

_ 4

4/m

422

4mm

_ 42m

4/mmm

R P 3

Hexagonal

Rhombohedral (trigonal)

Tetragonal (quadratic)

Orthorhombic

Monoclinic

1

_ 1

_ 3

32

3m

_ 3m

P _ 6

6/m

622

6mm

Cubic

6

23

_ m3

432

_ 43m

_ m3m

_ 62m

6/mmm P I F

Figure 5.17b: The 32 crystallographic point groups arranged by crystal system: stereographic projection of the equivalent directions. The rightmost column indicates the Bravais modes consistent with each of the systems.

104

Symmetry and Physical Properties of Crystals

The arrangement of entries on the four ﬁrst rows is such that the crystal lattices are ranked in order of growing symmetry (triclinic, monoclinic, orthorhombic, tetragonal), easy to identify since the point group of a crystal lattice is a subgroup of the point group of the crystal lattice on the next row. Group ¯1 of the triclinic lattice is a subgroup of group 2/m of the monoclinic lattice, which itself is a subgroup of group mmm (orthorhombic lattice), while the latter is a subgroup of 4 ⁄ m mm (tetragonal lattice). We note that, to determine the row corresponding to a given point group, we look for the holohedral group with the lowest symmetry of which it is a subgroup: for example point group mm2 is a subgroup of the holohedral group mmm of the orthorhombic lattice. It is also a subgroup of point group 4 ⁄ m mm of the tetragonal lattice, but a crystal with point group mm2 has an orthorhombic, not a tetragonal, crystal lattice. It may occur, under speciﬁc temperature or pressure conditions, that a crystal with point group mm2 happens to have two lattice parameters equal, for example a = b. Such a crystal is then accidentally tetragonal. The rhombohedral and hexagonal lattices appear on the following rows. The point group of the rhombohedral lattice is a subgroup of that of the hexagonal lattice. We make an important note: we will show in Chapter 6 that the crystals with point group 3, ¯3, 32, 3m and ¯3m, all shown on the 5th row, can have either a rhombohedral crystal lattice (noted R) or a hexagonal crystal lattice (noted P). This is indicated by the two arrows pointing from this row to the rhombohedral and hexagonal lattices, as well as by the P associated to R in the column showing the Bravais modes. The cubic groups are shown on the last row. If the point group of the crystal is a subgroup of the holohedral group, the group is said to be merohedral. The table below shows the type of merohedry as a function of the ratio between the order of the holohedral group nH , viz. the order of the symmetry group of the crystal lattice, and the order of the merohedral group nM of the crystal. nH /nM

Designation of the group

1

holohedral

2

hemihedral

4

tetartohedral

8

ogdohedral

We recall the rules, already stated in Sections 5.4.2 to 5.4.4, of the HermannMauguin notation. A mirror parallel to an n-fold (or n ¯ -fold) axis is noted through an m next to the n (or n ¯ ), and a mirror perpendicular to an n-fold axis by an m as a denominator. For example group 3m involves a 3-fold axis

Chapter 5 – Point groups

105

and three mirrors parallel to this 3-fold axis. Group 4/m has a 4-fold axis and a mirror perpendicular to it. For the cubic groups, the ﬁrst symbol shows the order of the axes parallel to the cube axes (2 or 4) or the existence of mirrors perpendicular to these axes (m). The second symbol shows the existence of 3-fold axes parallel to the major diagonals of the cube, or ¯3 if there is also an inversion center. The third symbol, if it exists, shows the existence of 2-fold axes parallel to the diagonals of the cube faces or of mirrors perpendicular to these directions. Figure 5.17a also shows, next to this nomenclature which is the usual one for crystallographers, the Schönﬂies notation, frequently used in group theory, and summarized below: For all groups except for the cubic groups and groups ¯4 and m: ﬁnd the axis with the highest order, call it n, and assume it is vertical, associate to this group its cyclic (Cn ) or dihedral (Dn ) subgroup with the highest order, and start the notation with Cn or Dn respectively. This notation is complemented, if necessary, with a subscript i if there is also a center of inversion one of the following subcripts if there are mirrors: h if the mirror is horizontal, v if it is vertical and there is no horizontal 2-fold axis, or if there is a horizontal 2-fold axis in the plane of the mirror, d if the mirrors are vertical with 2-fold axes in the bisecting planes of the mirrors. Example: group 4mm, with subgroup C4 , has a vertical mirror as an extra generating element. It is noted C4v . The other notations are the following: notation Sn refers to the presence of a rotoinversion axis n ¯ , but it is used only for group S4 (¯4), because group ¯3 ¯ is noted as C3i (a 3-fold axis being equivalent to a 3-fold axis and a center of symmetry), and group ¯6 is noted C3h (a ¯ 6-fold axis being equivalent to a 3-fold axis and a mirror perpendicular to it). The notation Cs indicates group m (the s is from the German word Spiegel = mirror). The notations T (tetrahedron) and O (octahedron) are used for the cubic groups. T is the group of the rotations of the tetrahedron (group 23). It is easy to check, with the help of Figure 5.17b, that adding a horizontal mirror to group 23 yields group m¯3, therefore noted Th , while adding a mirror in the diagonal planes gives group ¯43m, noted Td . Group O is the group of the rotations of the cube (group 432), which becomes Oh (m¯3m) if a horizontal mirror is added.

106

Symmetry and Physical Properties of Crystals

5.7. Laue classes The investigation of X-ray diﬀraction by crystals shows that the intensity of the beams diﬀracted by a given crystal is the same whether the reﬂection3 occurs oﬀ one side or the other of the lattice planes. This result, known as Friedel’s law, only breaks down when the wavelength of the radiation is very near an absorption edge, i.e. when the energy of an X-ray photon is equal or nearly equal to that of an electronic energy level of one of the atoms in the crystal. Away from the absorption edges, diﬀraction thus introduces a center of symmetry even if the crystal structure has none. This is why the 32 symmetry groups are arranged into 11 sets such that the eﬀects of the crystal symmetry on diﬀraction are the same within each set. Each of the 11 centrosymmetric crystallographic groups deﬁnes one of these sets, called Laue classes. For any of the 21 remaining groups, just multiplying the group with (E, I) produces the centrosymmetric group which deﬁnes the Laue class to which it belongs. We thus obtain Table 5.2. Table 5.2: The 11 Laue classes. Each class is surrounded by a thick line. 1

– 1

2

m

2 — m

222

mm2

mmm

4

– 4

4 — m

422

4mm

3

– 3

32

3m

– 3m

6

– 6

6 — m

622

6mm

23

– m3

432

– 43m

– m3m

– 42m

4 — mm m

– 62m

6 — mm m

3. Crystal diﬀraction can be described, as in Section 3.2.1, through the condition that the scattering vector be a reciprocal lattice vector h∗ = ha∗ + kb∗ + lc∗ where a∗ , b∗ , c∗ are the basis vectors of the reciprocal lattice. It is often convenient to describe it as mirror reﬂection oﬀ the lattice planes (hkl), but selective reﬂection because it only occurs when the wavelength satisﬁes Bragg’s law. This is why crystal diﬀraction is often referred to as Bragg reﬂection.

Chapter 5 – Point groups

107

5.8. Plane point groups It is useful, both for later discussions on lattices, and for surface crystallography, to determine the plane crystallographic groups. Their determination can be performed in the same way as for 3-dimensional groups, by looking for the proper groups, then the improper groups. The operation of symmetry with respect to a given point O in the plane is identical to a rotation by 180◦ around an axis perpendicular to the plane that goes through O. It is no more an improper operation. The basic improper operation is now the operation of symmetry with respect to a plane perpendicular to the plane of the object, or mirror operation, noted m. All the plane symmetry elements are perpendicular to the reference plane. The only proper plane crystallographic groups are 1, 2, 3, 4, 6. The improper groups are obtained by multiplying these proper groups with group (E, m). We then obtain groups m, 2m or mm,4 3m, 4m, 6m. We note that these 10 plane crystallographic point groups are identical to 10 of the 3-dimensional point groups.

5.9. Isotropy point groups The investigation of the physical properties of crystals will beneﬁt from a generalization of the discussion in this chapter to inﬁnite-order non-crystallographic point groups. These are groups featuring an axis of revolution, which is none other than an inﬁnite-order axis, or isotropy axis. It will be performed according to the same rules. The result is given below. For each of these groups, we give an example of an object with the symmetry elements of the group (Fig. 5.18).

Proper groups (a) There is a single isotropy axis, and no other symmetry operation. The group has for its symbol ∞. It corresponds to the cyclic groups (Sect. 5.4.2). This is the symmetry of a half cone rotating around its axis. (b) There is a single isotropy axis and an inﬁnity of 2-fold axes perpendicular to it. This group is noted ∞2, and it corresponds to the dihedral groups of Section 5.4.3. This is the symmetry of two half-cones with the same apical angle and with the same axis, but opposed at the apex and rotating in opposite directions.

4. This group contains the symmetry operations associated to a 2-fold axis and a mirror going through this axis. The existence of these two symmetry elements entails the existence of another mirror going through the axis and perpendicular to the ﬁrst one. This is why this group is usually called mm.

108

Symmetry and Physical Properties of Crystals

2

— m

m — m

— m— m

m

(a)

(b)

(c)

(d)

(e)

(f)

(g)

Figure 5.18: Examples of objects having the symmetry of each of the 7 isotropy groups (c) There is an inﬁnity of isotropy axes. This group, noted ∞ ∞, is the limiting case of groups involving several axes of order larger than 2 (corresponding to the cubic proper groups of Sect. 5.4.4). This is the symmetry of a sphere containing a liquid featuring rotatory power, hence not superimposable with its mirror image.

Improper groups containing inversion We multiply by (E, I) the groups obtained in (a), (b) and (c). Since these groups contain at least one isotropy axis (which therefore includes a 2-fold axis), the presence of the center of symmetry is equivalent to the existence of a mirror perpendicular to the axis. We obtain: (d) one isotropy axis and a perpendicular mirror, i.e. the group ∞/m (corresponding to groups 2/m, 4/m, 6/m). This is the symmetry of a cylinder rotating around its axis, and also that of an axial vector (Sect. 10.6.1). (e) one isotropy axis, an inﬁnity of mirrors going through this axis, and a mirror perpendicular to the axis (and a center of symmetry). This group is called ∞/mm (it can be associated to groups 4 ⁄ mmm and 6 ⁄ mmm). This is the symmetry of a stationary cylinder. (f) an inﬁnity of isotropy axes, an inﬁnity of mirrors (and a center). This group is noted ∞/m ∞/m. This is the symmetry of a sphere.

Improper group which does not contain inversion (g) Group ∞2 admits group ∞ as its half order subgroup. The process described for the crystallographic groups now reduces to replacing the inﬁnity of 2-fold axes by an inﬁnity of mirrors going through the isotropy axis. This group is called ∞m. It generalizes the pyramidal groups. This is the symmetry of a stationary half-cone, and also that of a polar vector (Fig. 9.2).

Chapter 5 – Point groups

109

These groups can be classiﬁed into two systems: the cylindrical system, which contains a single axis of revolution (a, b, d, e and g) and the spherical system which contains an inﬁnity of axes of revolution (c and f). These inﬁnite-order groups will be used in the second part of the book to characterize the symmetry of some physical quantities. For example an electric ﬁeld has for its symmetry group ∞m, a magnetic ﬁeld ∞/m and a uniaxial stress (which will be deﬁned in Sect. 11.5.1) ∞/mm.

5.10. Exercises Exercise 5.1 Consider two axes x x and y y, intersecting at point O, and enclosing an angle θ. Let A be the operation consisting of a rotation by π around x x and A the operation rotation by π around y y. 1.

Show that the product A A is equal to a rotation by 2θ around an axis that goes through O and is perpendicular to the plane Π formed by x x and y y. Denote this operation as R⊥ (2θ).

2.

Deduce that A = R⊥ (2θ)A and A = A R⊥ (2θ), so that, if an object features an n-fold axis and a 2-fold axis perpendicular to it, then it also features n 2-fold axes with angles π/n between them.

Exercise 5.2 Consider the point group 32, i.e. a group comprising the symmetry operations associated to a 3-fold axis and to a 2-fold axis perpendicular to it. Draw the stereographic projection, onto a plane perpendicular to the 3-fold axis, of the directions equivalent to a general direction through these symmetry operations. Deduce that this group includes three 2-fold axes perpendicular to the 3-fold axis, with angles of 2π/3 between them. This is an easy way of retrieving the result of the preceding exercise in the special case where n = 3. It can be easily generalized to any value of n. Exercise 5.3 1.

Show that the existence of two intersecting and perpendicular 4-fold axes leads to the existence of four 3-fold axes parallel to the major diagonals of a cube with sides parallel to the 4-fold axes. The derivation can be made either using the rotation matrices representing the symmetry operations, or by considering a cube ABCDEFGH and submitting it to the successive operations.

2.

Show that the reciprocal proposition is not true. The existence of four 3fold axes along the major diagonals of a cube does not entail the existence of three 4-fold axes parallel to the sides of the cube. It only entails the existence of 2-fold axes parallel to the cube sides.

110

Symmetry and Physical Properties of Crystals

Exercise 5.4 Consider Figure 5A.5b showing the stereographic projection of some of the symmetry elements of a cube. If the projection plane is perpendicular to the basis vector c of a cubic lattice, and if b is the projection of [100], the circular arcs b Fb and b F b are the projections of the diagonal plane (01¯1). Show that the centers of the circles to which these arcs belong are points a and a respectively. √ Note: it may be helpful to note that tan π8 = 2 − 1, a value which can be 2 tan θ π retrieved using tan 2θ = 1−tan 2 θ and tan 4 = 1. Exercise 5.5 Consider the various point groups consistent with a hexagonal lattice, and rank them according to their merohedry. Figure 5.17b can be useful. Exercise 5.6 A form {hkl} of a crystal comprises the set of faces in this crystal which are equivalent to face (hkl). 1.

Give the Miller indices of the various planes in the form {31¯40} for crystals with point group (a) 6mm, then (b) ¯62m.

2.

Same question for form {111} in crystals belonging to the various cubic groups.

Chapter 5 – Point groups

111

Appendix 5A. Complements on the stereographic projection 5A.1. Stereographic projection of the transform of a given direction through the symmetry operations associated to various symmetry elements The notations are as follows. We call Ov the starting direction. It intersects the sphere at P, the stereographic projection of which is called n. Direction Ov , the transform of Ov through the considered symmetry operation, cuts the sphere at P , and its stereographic projection is called n . The meridian half-planes containing OP and OP intersect the projection plane along OQ and OQ respectively (Fig. 5A.1). Projections n and n are then located on OQ and OQ respectively. v’ N

N

Q’

P’

v P O

n

n’ Q

O

n’

Q’

O n Q

S

S

(a)

(b)

(c)

Figure 5A.1: Illustrating the notations used in this appendix: (a) meridian plane of the initial direction Ov ; (b) meridian plane of direction Ov , the transform of Ov through the symmetry operation; (c) stereographic projections n and n of directions Ov and Ov 5A.1.1. n-fold axis perpendicular to the projection plane The projection of the axis consists of two points coinciding with the origin O. The meridian planes containing Ov and Ov enclose an angle 2π/n. Ov and Ov are at the same angle θ to NS and On = On . Projection n is the transform of n through a rotation by 2π/n around an axis perpendicular to the projection plane and going through O (Fig. 5.2 and 5.4). 5A.1.2. Mirror coinciding with the equatorial plane The stereographic projection of the mirror is the equatorial circle. The meridian plane containing Ov transforms into itself in the mirror operation, and in this plane Ov and Ov are symmetric with respect to the trace of the equatorial plane (Fig. 5A.2a). The projections coincide but they are represented by diﬀerent signs since Ov and Ov are in two diﬀerent hemispheres (Fig. 5A.2b).

112

Symmetry and Physical Properties of Crystals N v P n n’

O

n’ n

7

O

QQ’ P’

Q

v’

S

(a)

(b)

Figure 5A.2: (a) Meridian plane containing a general direction Ov and its transform Ov through symmetry with respect to a mirror coinciding with the equatorial plane; (b) stereographic projections of the mirror (thick line) and of directions Ov and Ov 5A.1.3. Mirror going through axis NS The projection of the mirror is the line AB, intersection of the mirror and the equatorial plane (Fig. 5.3b). The meridian plane containing OP is symmetric of the one containing OP with respect to the mirror plane. In each of these planes, OP and OP enclose the same angle θ with axis NS, so that On = On . Their stereographic projections n and n are therefore symmetric with respect to the stereographic projection of the mirror. 5A.1.4. 2-fold axis in the equatorial plane The projection of the axis consists of two opposite points on the equatorial circle, A and B (Fig. 5A.3c). Direction Ov intersects the sphere at point P, which projects on the equatorial plane at H. The meridian plane containing Ov is at an angle ϕ with AB. The transform of this meridian plane through a rotation by π around AB is a meridian plane enclosing the same angle ϕ with AB. The transforms of P and H are P and H respectively, and it is easy to show, using Figure 5A.3a, that (OH, OP) = (OH , OP ) = β, P being in the northern hemisphere and P in the southern hemisphere. The stereographic projections n and n are therefore at the same distance from O on OQ and OQ (Fig. 5A.3b), both of which enclose with AB the angle ϕ. They are represented with diﬀerent symbols (Fig. 5A.3c).

5A.2. Stereographic projections of the symmetry elements of a cube 5A.2.1. Preamble We look for the stereographic projection of a plane going through the center O of the sphere and which does not go through axis NS. Its intersection with the sphere is a major circle Γ which intersects the equatorial circle at a and a (Fig. 5A.4a).

Chapter 5 – Point groups

113

v P C

A

O

H

Q A2 axis B

H’

P’

Q’ v’

(a) N

Q’ H’

n’

N

OO

P

n

H

Q

v

n O

A

n’

v’ P' S

Q B Q’

S

(b)

(c)

Figure 5A.3: Construction of the stereographic projection of the transform of a general direction Ov through rotation by π around an axis A2 located in the equatorial plane: (a) perspective view; (b) meridian planes containing Ov and Ov ; (c) stereographic projection

N 2 a’

O

a

C

a’

a

1

S (a)

(b)

Figure 5A.4: A plane which does not go through axis NS. (a) Perspective view. (b) The stereographic projection of the plane consists of two arcs in full and dotted thick line, going through a and a .

114

Symmetry and Physical Properties of Crystals

The stereographic projection of a circle being a circle, the projection of Γ starting from the south pole is a circle Γ1 going through a and a (Fig. 5A.4b). This circle has two parts: arc aa’ (thicker line), located in the equatorial disk C, which corresponds to the projection of the half major circle located in the northern hemisphere. The second half of major circle Γ, located in the southern hemisphere, must be transformed through an inversion with the north pole as pole. The transform of Γ through the north pole inversion is circle Γ2 , symmetric of Γ1 with respect to aa , with only the circular arc contained in the equatorial disk retained. It is represented in dotted line to indicate that it is the image of an arc in the southern hemisphere. 5A.2.2. Cubic groups The stereographic projection is performed onto a plane parallel to one cube face, for example face HJKL of the cube shown on Figure 5A.5a. 1.

Stereographic projection of one of the A3 axes of the cube Select for example the A3 axis coinciding with the major diagonal HK . This diagonal is at the intersection of two diagonal planes of the cube, HJK L and HLK J . The stereographic projection of plane HJK L consists of two arcs intersecting along diameter aa parallel to HJ. That of plane HLK J consists of two arcs intersecting along bb parallel to side HL (Fig. 5A.5b). The stereographic projections of the axis are the intersections of the stereographic projections of the two diagonal planes, i.e. point F is in the northern hemisphere and point F in the southern hemisphere. They are represented by their characteristic symbol (an equilateral triangle). Axis A3 is contained in a third diagonal plane of the cube, HKK H . This plane goes through axis NS. Its projection coincides with its intersection with the projection disk, i.e. the segment cc at 45◦ to aa and bb . It goes through F and F .

2.

Stereographic projection of all the symmetry elements of the cube, i.e. of the point group m¯3m (Fig. 5A.5c) The three A4 axes represented by their characteristic symbols. The mirrors perpendicular to these A4 axes, i.e. the mirror parallel to the projection plane (and to face HJKL), the projection of which is the equatorial circle itself, and the mirrors parallel to axis NS, the projections of which are the segments aa and bb (mirrors parallel to HJJ H and JKK J respectively). The diagonal mirrors. There are six of them. We investigated three of them, which intersect along an A3 axis. To each of these three mirrors we can associate another diagonal mirror which is perpendicular to it and intersects it along an A4 axis. For example, mirror LJJ L is associated to mirror HKK H . These two mirrors go through axis NS and their stereographic projections are cc and dd . Mirror H J KL is

Chapter 5 – Point groups

115

associated to HJK L . They are symmetric of each other with respect to the projection plane. Their stereographic projections are identical (arcs aFa and aF a ), but with the characteristic symbols reversed. The arc in full line of one is superimposed on the arc in dotted lines of the other, and vice-versa. Finally the full lines cover the dotted lines. The same applies to the projections of the diagonal mirror HLK J and H L KJ, which consist of the arcs bFb and bF b . Six A2 axes perpendicular to the diagonal mirrors, and therefore located in the associated diagonal mirror. They connect, within these mirrors, the middles of two opposite sides. For example MP, located in the diagonal mirror HJK L , is the A2 axis perpendicular to mirror H J KL. Its stereographic projection consists of two points G and G’ (Fig. 5A.5b). The axis A2 located in the mirror H J KL projects on the same points but with diﬀerent symbols. On the general ﬁgure, we show these two axes (as well as the four others) using the representative symbols of 2-fold axes. A center of symmetry. Its stereographic projection is at the center of the projection disk. Furthermore, the presence of a center of symmetry changes the A3 axes into ¯3-fold axes. L’

P K’

H’ O

J’

L K

H M

J

(a) b’

b’ d’

c’ G

a F’

c’

F G’

c

a’

a

a’ d

c b (b)

b (c)

Figure 5A.5: (a) Perspective view of a cube; (b) stereographic projection of some of its symmetry elements and (c) of all its symmetry elements

Chapter 6

Bravais lattices This chapter shows how the Bravais lattices, already introduced in a qualitative way in Section 3.7, are enumerated. It can be skipped on ﬁrst reading.

6.1. Introduction Bravais lattices were introduced in Section 3.7. We showed that, in some cases, a multiple (or centered) cell evidences symmetry elements of the lattice which fail to appear in any primitive cell. We listed the 14 Bravais lattices (Sect. 3.7.2 and Tab. 3.3), without deriving how they are enumerated. The aim of the present chapter is to show how they are obtained logically. It can therefore be skipped on ﬁrst reading. The derivation rests on the result obtained in Section 4.3, namely that the symmetry operations of the point group of the crystal form a subgroup of the symmetry operations of the crystal lattice. The aim is therefore to ﬁnd out what type of crystal lattice is consistent with each of the 32 point groups. However, since all crystal lattices feature centers of symmetry (on the nodes, at the centers of the unit cells and in the middle of the vectors connecting neighboring nodes), the point symmetry group of a crystal lattice necessarily contains inversion. It is therefore suﬃcient to know the lattice types consistent with each of the 11 centrosymmetric point groups, each of which is characteristic of its Laue class, deﬁned in Section 5.7. The lattices of the 21 other groups are obtained by considering, for a given group, the group representative of its Laue class, i.e. the supergroup obtained by multiplying it with the group (E, I). This supergroup is one of the 11 centrosymmetric groups for which we determined the compatible lattice. In practice, we will use this remark only in the course of the derivation, because it is simpler to start out by determining which lattice is consistent with a low-symmetry point group. We will see that we reach a lattice for which the point group is much more symmetric than the starting group, and therefore necessarily includes a set of subgroups. Before that, it is necessary and illuminating to enumerate the plane lattices. The results obtained are no surprise; they were already given without derivation in Section 3.4.1.

© Springer Science+Business Media Dordrecht 2014 C. Malgrange et al., Symmetry and Physical Properties of Crystals, DOI 10.1007/978-94-017-8993-6_6

117

118

Symmetry and Physical Properties of Crystals

6.2. Plane lattices We recall that the 10 plane point groups are the groups 1, 2, 3, 4, 6, m, mm,1 3m, 4m, 6m (Sect. 5.8). We will investigate successively the plane lattices compatible with the low-symmetry point groups, viz. groups 1, 3, 4 and m. The results obtained make it possible to determine the plane lattices consistent with each of the 10 groups.

6.2.1. Group 1 The point group of any (general) plane lattice features a center of symmetry, i.e., in terms of plane groups for which the symmetry elements are normal to the plane, a 2-fold axis. The unit cell is a general parallelogram, a result valid for groups 1 and 2.

6.2.2. Group 3 Let a be the smallest of all lattice translations. Through a rotation by 2π/3 around the 3-fold axis, vector a becomes vector b (Fig. 6.1a). Vectors a and b deﬁne a primitive cell, since there cannot be a node within this parallelogram, or else a would not be the smallest lattice vector. Only one type of plane lattice is consistent with a 3-fold axis. Its primitive cell is a parallelogram with apical angles 2π/3 and π/3, and the lattice is called hexagonal. The symmetry of this lattice is 6m and the point groups consistent with this lattice are thus 3, 3m, 6, 6m (Fig. 6.1b).

b

120°

O

a b

120°

a

(a)

(b)

Figure 6.1: Plane lattice with point group 3: (a) primitive cell; (b) lattice, evidencing six concurrent mirrors, the trace of which is indicated by dotted lines

1. We saw that this notation is equivalent to the notation 2m.

Chapter 6 – Bravais lattices

119

6.2.3. Group 4 The same argument (rotation by 2π/4 = π/2 of the smallest lattice vector a, leading to vector b deﬁning, together with a, a square unit cell within which there can be no extra node) leads to a square primitive cell. The plane lattice, with square primitive cell, has point symmetry 4m and is consistent with the point groups 4 and 4m.

6.2.4. Group m Let a be a translation of the plane lattice that is neither parallel nor perpendicular to the trace uu of the mirror on the plane of the lattice, and b the transform of a in the mirror operation m (Fig. 6.2a). Translations a + b and a − b deﬁne orthogonal rows, respectively parallel and perpendicular to the mirror. Let a and b be the smallest lattice vectors along these directions (Fig. 6.2b). They deﬁne a rectangular unit cell for which one of the apices is noted O. Consider a lattice vector n starting from O and for which the end M is inside the rectangle deﬁned by the vectors a and b with origin O. Let n = OM be its image through operation m. Draw the vector n + n , parallel to b. By construction, it is smaller than 2b and can only be a multiple of b, i.e. 0 or b. In the same way, n − n can only be 0 or a. u’

a’ + b’ b’

a’

b M

M’ n’

a’ – b’

O

n a

u

(a)

(b)

Figure 6.2: Plane lattice with point group m. uu’ is the trace of one of the mirrors. Consider the various possible cases: 1.

n + n = 0 and n − n = 0, i.e. n = n = 0. The rectangular unit cell with basis vectors a and b is primitive.

2.

n + n = b and n − n = a, i.e. n = (a + b)/2. The rectangular unit cell is double. It is a centered unit cell.

3.

n + n = b and n − n = 0, i.e. n = b/2 or n + n = 0 and n − n = a, i.e. n = a/2.

120

Symmetry and Physical Properties of Crystals

These two solutions must be rejected because they contradict the starting assumption (a and b the smallest lattice vectors along these directions). These two plane lattices, with the rectangular unit cell respectively primitive and centered, have point symmetry mm, and the compatible crystal groups are m and mm.

6.2.5. Conclusion The survey of plane lattices is ﬁnished because, by searching for the lattices associated with the lowest symmetries, we have determined lattices with higher symmetry which ﬁnally include all the plane point groups. The results are gathered in Table 6.1. Table 6.1: Point groups consistent with the various plane lattices Plane lattice

Compatible point groups

Oblique

1, 2

Hexagonal

3, 3m, 6, 6m

Square

4, 4m

Rectangular Primitive (p) Centered (c)

m, mm

6.3. 3-dimensional lattices 6.3.1. Group 1 This group features no symmetry element. It is therefore consistent with a general parallelepiped-shaped primitive cell. The lattice is called triclinic. As for all lattices, it involves centers of symmetry and its point group is thus ¯1. It is therefore consistent with crystals with point groups 1 and ¯1.

6.3.2. Group 2 We showed (Sect. 3.3.4) that any rotation axis is parallel to a row of the direct lattice and perpendicular to a lattice plane. Consider row zz parallel to the 2-fold axis, and going through a given lattice node O. Let P0 be the lattice plane which is perpendicular to this row and goes through O (Fig. 6.3). In plane P0 , the primitive cell is a general parallelogram. Let a and b be two vectors deﬁning this unit cell. Let P1 be one of the two lattice planes parallel to P0 and closest to P0 . The lattice nodes in this lattice plane project onto P0 at the rate of one node per plane unit cell in P0 . Let F be the projection of one of these nodes, located in

Chapter 6 – Bravais lattices

121 z’

F

P1

b a

n B P0

O

F’

A

D

z

Figure 6.3: Three-dimensional lattice for a crystal with point group 2. zz is a 2-fold axis. P0 and P1 are two consecutive lattice planes. Vector n = OF connects node O in P0 to a node of plane P1 such that its projection is inside the plane unit cell OADB. one of the unit cells containing lattice node O, and let F be the node associated to it in P1 . F can also be located on the edges OA and OB of this unit cell, but A and B are excluded: if F were at A (or B) we would consider OF − a (or OF − b) and F would then be at O. Let us note vector OF as n. The three vectors a, b and n deﬁne a primitive cell. Let n be the lattice vector resulting from the transformation of n through a rotation by π around the 2-fold axis (Fig. 6.4a). The component n// of n, parallel to the axis, is conserved in the rotation, and the component n⊥ is transformed into −n⊥ . Also, n − n is a lattice vector. We obtain: n = n// + n⊥ ,

n = n// − n⊥ ,

n − n = 2n⊥ = pa + qb

(p and q integers)

Hence n⊥ =

q p a + b. 2 2

(6.1)

Taking into account the assumption we made about F and F , p/2 and q/2 are less than 1. Two cases must be considered: 1.

n⊥ = 0 (p = q = 0), so that n is perpendicular to P0 . The unit cell is a right prism with general parallelogram base. It is a primitive cell and the lattice is called monoclinic primitive.

2.

n⊥ = a/2 or n⊥ = b/2 or n⊥ = (a + b)/2. These three cases are equivalent, since nothing basically distinguishes lattice vectors a, b and a + b, any one of which can be chosen as a basis vector for a plane primitive cell in P0 .

Assume that n⊥ = a/2 (Fig. 6.4b). Plane P2 , parallel to P0 and P1 and located immediately above P1 , deduces from P0 through translation 2n, i.e.

122

Symmetry and Physical Properties of Crystals z’

z’ c = 2n F

n

n n’

2n F n b

b n a

O

F’

P0

O a/2 F’ a P0

z

z

(a)

(b)

Figure 6.4: Search for the lattice of a crystal with point group 2. (a) Vector n transforms into n by rotation around the 2-fold axis zz . (b) The situation when the component n⊥ of n perpendicular to zz is equal to a/2. 2n = 2n// + a, which is equal to 2n// modulo the lattice translations. The vectors a, b and c = 2n// deﬁne a monoclinic unit cell. This unit cell contains node F at the center of the rectangular face (a, c = 2n// ). It is a double unit cell, called base-centered monoclinic. The centered faces are parallel to the 2-fold axis. If, as we just did, we call c the basis vector parallel to the 2-fold axis, the lattice is called monoclinic B if the centered faces are (a, c), or monoclinic A if the centered faces are (b, c). If, as is still frequently the case, the basis vector parallel to the 2-fold axis is called b, the lattice is C or A depending on whether faces (a, b) or (b, c) are centered. The point group of a monoclinic lattice is 2/m. It is consistent with subgroups 2 and m and with group 2/m.

6.3.3. Group 3 In the lattice planes perpendicular to the 3-fold axis, the lattice is hexagonal. It is deﬁned by vectors a and b, with the same length and enclosing an angle 2π/3. The same argument as above leads to considering a lattice plane P0 perpendicular to the 3-fold axis, and its nearest neighbor P1 , which is parallel to it. Let n be the lattice vector connecting lattice node O in plane P0 to lattice node F located in P1 and which projects onto P0 inside a primitive plane unit cell containing O, or one of its sides OA and OB, excluding A and B. Let n be the transform of n through the operation rotation by 2π/3 around the 3-fold axis going through O. The component n// of n parallel to the axis is conserved in the rotation. n = n// + n⊥ ,

n = n// + n⊥ ,

where n⊥ and n⊥ are respectively the components of n and n perpendicular to the 3-fold axis (Fig. 6.5).

Chapter 6 – Bravais lattices

123 B

D b F’

n

n’ O

a

A

Figure 6.5: Primitive cell in plane P0 perpendicular to the 3-fold axis Taking into account the assumption made about F , the end of n⊥ is located inside the parallelogram OADB (or on OA or AB, excluding A and B) and thus its norm is smaller than a. We have ||n⊥ || < a. Since n⊥ − n⊥ =

√

√ 3 n⊥ , we obtain n⊥ − n⊥ < a 3.

As n − n is a lattice vector, n⊥ − n⊥√ , which is equal to it, is also a lattice vector, the norm of which is less than a 3. This norm can therefore have only two values, 0 or a. 1.

n⊥ − n⊥ = 0, so that n⊥ = n⊥ = 0. Vector n is perpendicular to P0 and the unit cell is a right prism whose base is an isosceles parallelogram with apical angle 2π/3. The unit cell is primitive, and the lattice is called hexagonal primitive. The point group of such a unit cell is 6/mmm, of which 3 is a subgroup (of index 8). The hexagonal lattice is therefore consistent also with groups 3, ¯3, 32, 3m, ¯3m, 6, ¯6, 6/m, 622, 6mm, ¯62m, subgroups of 6/mmm. This result was shown on Figures 5.17a and 5.17b.

2.

n⊥ − n⊥ = a, and then n⊥ − n⊥ is a lattice vector in P0 , with length a. It is therefore equal to a or b or a + b. Assume it is equal to a (Fig. 6.6a). The end F of n⊥ is then at the center M of the equilateral triangle OAD, and the nodes of the plane lattice P1 project at M and at all the points deduced from M through lattice translations a and b, thus, for example, at N and P. The lattice of plane P2 , immediately above P1 , deduces from the lattice of plane P0 through translation 2n = 2n// + 2n⊥ , and its nodes project onto P0 at N, such that ON = 2OM, and at all the points deduced from N through the lattice translations, for example at Q, R and S.

The lattice in plane P3 immediately above P2 is deduced from that of P0 through translation 3n = 3n// + 3n⊥ . But 3n⊥ = OK, a lattice vector equal to 2a + b. The nodes of plane P3 project on the nodes of P0 . Comparing Figures 6.6a and 3.14c, we see that the unit cell is a rhombohedron (Fig. 6.6b), i.e. a parallelepiped for which the basis vectors a , b and c have the same length, and for which the major diagonal LT is a 3-fold axis. All its faces are lozenges, equal to one another. The point group of a rhombohedral unit cell is ¯3m. Such a lattice is therefore consistent with the point group ¯3m and its subgroups 3, ¯3, 32, 3m.

124

Symmetry and Physical Properties of Crystals T B

D b

N

K N

R

n’ O

n a

S

R’

S’

M A

N’

Q

M’

P’ c’

P

Q’

a’

b’

L

(a)

(b)

Figure 6.6: Rhombohedral lattice: (a) projection onto plane P0 of the lattice nodes; (b) rhombohedral unit cell. P , M , N are in plane P1 and project onto P0 at P, M and N (crosses); Q , R , S are in plane P2 and project onto P0 at Q, R and S (empty circles); T is in plane P3 and projects at O (full circle). We thus obtained the two following results: 1.

¯ 32, 3m and ¯3m are consistent with a The crystals with point group 3, 3, primitive rhombohedral crystal lattice, noted R, and also with a primitive hexagonal lattice, noted P. Some crystals with one of these point groups have a rhombohedral lattice while others have a hexagonal lattice. For example, crystals of calcite CaCO3 , with point group ¯3m, have a rhombohedral lattice while crystals of Ca(OH)2 , with the same point group, have a hexagonal lattice.

2.

The hexagonal lattice is consistent with groups 6, ¯6, 6/m, 622, 6mm, ¯62m and 6/mmm. It will therefore not be necessary to examine group 6.

6.3.4. Group 4 Plane P0 , perpendicular to the 4-fold axis, is a lattice with a square primitive cell, with basis vectors a and b with the same norm a. The same argument as for groups 2 and 3 leads to considering the vector n connecting lattice node O in P0 to node F in lattice plane P1 (parallel to P0 and nearest neighbor to it) which projects onto P0 at point F (Fig. 6.7a), located within the plane unit cell OADB (or on OA and OB, excluding A and B). Let n be the transform of n through rotation by π/2 around the 4-fold axis. The component n// of n parallel to the axis is conserved in the rotation. We have n = n// + n⊥ , and

n = n// + n⊥ n⊥ = n⊥ .

√ Also, the assumption made on F leads to n⊥ < a 2.

Chapter 6 – Bravais lattices

125

c = 2n B

D

B

b n’

b

n O

F’ a

(a)

Figure 6.7: (a) Plane P0 , n⊥ through a n⊥ − n⊥ = a. Thus and

n

F’ B

n

n’ A

F

D

O

a

D F’

A

O

A

(b)

Search for the lattice of a crystal with point group 4. perpendicular to the 4-fold axis: n⊥ is the transform of rotation by π/2 around the 4-fold axis. (b) Case where The end of vector n = OF is at the center of the unit cell. n − n = n⊥ − n⊥ √ n⊥ − n⊥ = n⊥ 2.

Therefore n − n , and n⊥ − n⊥ which is equal to it, are lattice vectors parallel to P0 with norm smaller than 2a. Two cases should be distinguished: 1.

n⊥ − n⊥ = 0, so that n⊥ = n⊥ = 0 and n = n = n// . The unit cell is primitive. It is a rectangle parallelepiped with square base. The unit cell is called tetragonal primitive.

2.

n⊥ − n⊥ = a so that n⊥ = (a + b)/2. There is a lattice node which projects at the center of the square plane unit cell OADB (Fig. 6.7b). The plane P2 , nearest neighbor to P1 , deduces from P0 through translation 2n = 2n// + a + b. The nodes of P2 therefore project on the nodes of P0 . The lattice has a tetragonal double unit cell, with a node at the center of the unit cell.

This is a tetragonal body-centered lattice, noted I. The point group of a tetragonal unit cell is 4/m mm. This unit cell is consistent with point groups 4, ¯4, 4/m, 422, 4mm, ¯42m and 4/m mm. A tetragonal unit cell can therefore be primitive (P) or body-centered (I). It is then unnecessary to deal with group 6, since it occurred in a natural way when considering group 3 (Sect. 6.3.3). The above discussions led to the determination of the lattices consistent with 24 of the 32 point groups. We now search for the lattice consistent with the least symmetric of the remaining point groups, viz. 222.

126

Symmetry and Physical Properties of Crystals

6.3.5. Group 222 This group features three 2-fold axes, perpendicular to one another. Each of these axes being parallel to a lattice row (Sect. 3.3.4), the unit cell, be it primitive or centered, is therefore a rectangle parallelepiped with basis vectors a, b, and c, orthogonal to one another. The lattice is called orthorhombic. Consider the 2-fold axis parallel to vector c. The lattice plane perpendicular to c has a rectangular unit cell which, as we saw in Table 6.1, can be either primitive or centered. We will therefore successively apply the result of Section 6.3.2 to each of these unit cells. The plane unit cell (a, b) is primitive (plane lattice p) The approach of Section 6.3.2 leads to the result given in Equation (6.1): n⊥ =

q p a + b. 2 2

Three cases must be considered: 1.

p = q = 0, so that n⊥ = 0. The unit cell is primitive.

2.

p = 1, q = 0 or p = 0, q = 1, so that n⊥ = a/2 or b/2. The lattice is base-centered B or A. The unit cell is double.

3.

p = 1, q = 1, so that n⊥ = (a + b)/2. The lattice is body-centered, i.e. I. The unit cell is double.

The plane unit cell (a, b) is centered (plane lattice c) We can choose as basis vectors of a primitive cell of the 2-dimensional lattice a and (a + b)/2. We then obtain n⊥ =

q p a + (a + b) 2 4

with p and q integers. The cases to be considered are: 1.

p = 0, q = 0 so that n⊥ = 0. The lattice is base-centered, with the centered base being (a,b), and the lattice is C-type.

2.

p = 1, q = 0, so that n⊥ = a/2. The face (a, c) is centered. Vector (a + c)/2 is a lattice translation. Since face (a, b) is centered, (a + b)/2 is also a lattice vector and, through addition modulo a lattice vector, so is (b+c)/2. All the faces are centered, and the lattice is face-centered (F) orthorhombic.

3.

p = 0, q = 1, so that n⊥ = (a + b)/4.

4.

p = 1, q = 1, so that n⊥ = (3a + b)/4.

Chapter 6 – Bravais lattices

127

Cases (3) and (4) are to be rejected, since they lead to lattices that do not accept a 2-fold axis parallel to a or b. In conclusion, the orthorhombic lattice can be primitive (P), base-centered (A, B or C), body-centered (I) or face-centered (F). The orthorhombic lattice has symmetry mmm, and it is therefore consistent with groups 222, mm2 and mmm.

6.3.6. Group 23 Among the remaining groups, the least symmetric one is group 23. It is a supergroup of 222, which means that it features all the symmetry operations of 222, with additional 3-fold axes. This implies that the lengths of basis vectors a, b and c are equal. We can therefore start out from the results obtained for 222, adding the equality of the lengths of a, b and c. The unit cell is a cube which can be primitive (P), body-centered (I) or face-centered (F). The A, B and C lattices are not consistent with the existence of 3-fold axes, and are therefore ruled out. The lattice is cubic. The point group of the lattice is m¯3m and the cubic lattice is consistent with groups 23, m¯3, 432, ¯43m and m¯3m. We have now gone through the full list of crystallographic point groups, and the overall result is shown in the last column of Figures 5.17a and 5.17b.

Chapter 7

Space groups After showing how the space groups are constructed, this chapter aims at enabling the reader to understand what the denomination of a given space group contains, and to eﬃciently use volume A of the International Tables for Crystallography. This volume lists all the space groups and gives many of their properties. The last section shows some examples of space groups.

7.1. Introduction We saw that the symmetry operations of a crystal can be expressed in the form (S, t) where S is a rotation or a rotoinversion about an axis going through a given point O, and t a translation. Point O is not explicitly mentioned in the notation because it is chosen as common to all the operations (S, t). We also saw that the symmetry of the physical properties of a crystal depends only on the operations S, which form a group, and, in Chapter 5, we enumerated the 32 symmetry groups of the operations S, called orientation groups or, more often, point groups. We must now enumerate the symmetry groups of the operations (S, t). The connection between the point group and the space group was established rigorously in Chapter 4. We recall it brieﬂy here. The group T of the lattice translations (E, n) where E is the identity operation and n a vector of the crystal lattice, n = ua + vb + wc (a, b and c are the basis vectors of the crystal unit cell and u, v, w any integers), is a subgroup of the group G of the symmetry operations of the crystal. We can decompose this group G into packets (or cosets), each of which is the product of an operation (Si , ti ) with all the translation operations, so that: G = T + T(S1 , t1 ) + T(S2 , t2 ) + T(S3 , t3 ) + . . . + T(Sm , tm ) = T(E, 0) + T(S1 , t1 ) + T(S2 , t2 ) + T(S3 , t3 ) + . . . + T(Sm , tm ). To perform this partition of G by the group T of lattice translations, we start by setting aside the group T. We choose among the remaining elements of G one operation (S1 , t1 ), and we perform all the products of this operation with © Springer Science+Business Media Dordrecht 2014 C. Malgrange et al., Symmetry and Physical Properties of Crystals, DOI 10.1007/978-94-017-8993-6_7

129

130

Symmetry and Physical Properties of Crystals

the lattice translations. This set T(S1 , t1 ) is then put aside, and the process is repeated until all the elements of G have been used. The vectors ti are deﬁned modulo the lattice translation vectors. We can therefore choose them either equal to zero, or equal to pa + qb + rc with p, q, and r smaller than 1. The set of the cosets T(Si , ti ) thus deﬁned forms Gs , the space group or position group of the crystal, which can also be written as: Gs = (E, 0) + (S1 , t1 ) + (S2 , t2 ) + (S3 , t3 ) + . . . + (Sm , tm ) (modulo T),1 by replacing each coset T(Si , ti ) by (Si , ti ) modulo T. The operations (Si , 0) obtained by replacing, in (Si , ti ), the translation ti by a zero translation, form the point group or orientation group G0 of the crystal: G0 = (E, 0) + (S1 , 0) + (S2 , 0) + (S3 , 0) + . . . + (Sm , 0). The 32 point symmetry groups compatible with the existence of a crystal lattice were enumerated in Chapter 5. The ﬁrst task in this chapter will be to determine the operations (Si , ti = 0) which can exist when the existence of the crystal lattice is taken into account. We will thus obtain the symmetry operations associated to screw axes and to glide mirrors. We will then show how the space groups can be determined starting from the point groups, but we will not enumerate them systematically. There are 230 of them. They are described in volume A of the International Tables for Crystallography (I.T. A) [1], presented in Section 7.3.3.

7.2. Enumeration of the operations (S, t) We considered till now symmetry operations of the form (S, t) where operations S are rotations (or rotoinversions) around an axis that goes through point O, chosen arbitrarily and common to all the symmetry operations. We showed (Sect. 4.2.1) that this choice of a common point for all the rotation and rotoinversion axes is possible because we may always replace an operation (S(O), t) by an operation (S (O ), t ) where O is any point, if S = S and t = t + (S – E) OO . We now reverse the reasoning, in order to determine whether it is possible, for any one of the operations (S(O), t), with common origin O, to displace the 1. Adding “modulo T” is mandatory in order for the above operations to form a group because it can happen that the product of two of the operations (Si , ti ) is equal to (Sj , tj + n) while, as mentioned above, the ti are smaller than lattice translations.

Chapter 7 – Space groups

131

origin to a point O so that we obtain an operation for which the translation part is zero, (S(O ), 0). To obtain t = 0 we require: t = (E – S) OO .

(7.1)

We will see that this equation can have solutions in some cases. When it does not, we will determine the values of t compatible with the existence of a crystal lattice. We will study separately the cases where S is a rotation (Sect. 7.2.1) ¯ (Sect. 7.2.2). and those where S is a rotoinversion, denoted as above with S

7.2.1. S is a rotation. Deﬁnition of screw axes It is easily shown that, if S is a rotation, the vector t deduced from relation (7.1) is perpendicular to the rotation axis. Rotation S(O) transforms vector OO into vector OO (Fig. 7.1). We obtain: t = (E – S) OO = OO − OO = O O

(7.2)

which is perpendicular to the rotation axis. Thus the translation part of the operation can be zero only if the initial translation t is perpendicular to the rotation axis. z’ O”

O’

O z

Figure 7.1: Rotation of a vector OO around an axis zz that goes through O The determination of the new position O of the axis which cancels the translation will be presented in Section 7.2.3. We now consider the case (S, t// ), where t is parallel to the rotation axis, so that the translation part can no more be canceled by a change in the position of the rotation axis. Suppose S is a rotation by 2π/q around a q-fold axis, and determine the operation product of this operation by itself. Using relation (4.8), valid for operations S1 and S2 having the same origin, which we reproduce below: (7.3) (S2 , t2 )(S1 , t1 ) = (S2 S1 , S2 t1 + t2 ). We obtain: (S, t// ) (S, t// ) = (S2 , St// + t// ).

132

Symmetry and Physical Properties of Crystals

But St// = t// since rotation of a vector parallel to the rotation axis transforms this vector into itself. We obtain (S, t// )2 = (S2 , 2t// ). Repeating this operation q times, we obtain: (S, t// )q = (Sq , q t// ) = (E, q t// ) which is necessarily a symmetry operation of the crystal. Since the rotation part is the identity operation, this symmetry operation is a lattice translation (E, n) and qt// = n. Vector t// is therefore parallel to a crystal row, which is no surprise since it is parallel to a symmetry axis (Sect. 3.3.4). Let c be the smallest lattice vector parallel to the q-fold axis we are discussing. qt// = mc

and

t// = mc/q

where m is any integer. There are q − 1 solutions: t// = c/q, t// = 2c/q, . . . , t// = (q − 1)c/q. The next values would be t// = c, a crystal lattice vector, and then vectors equal to the above ones modulo c. The symmetry elements associated to these operations, products of a rotation and a translation parallel to the rotation axis, are called screw axes (Sect. 2.2.4). Table 7.1 summarizes the various screw axes, their short notation, the translation to which they are associated, and the symbol that represents them. Table 7.1: Screw axes Order of the axis

2

3

4

6 6 61

64

Notation

2 21 3 31

Translation

0 c/2 0 c/3 2c/3 0 c/4 2c/4 3c/4 0 c/6 2c/6 3c/6 4c/6 5c/6

32

4 41

42

43

62

63

65

Symbol

Consider a crystal featuring a screw axis, and a given atom of this crystal which is not located on this axis. There are then atoms of the same nature at all the positions which deduce from the position of this atom through the various symmetry operations associated to this axis. The atoms are located on a helix or screw (hence the name screw axis), the axis of which is this screw axis. A helix or screw is a chiral object, i.e an object which is not superimposable to its mirror image.

Chapter 7 – Space groups

133

c

21

c

31

32 4’ 3

5 2

c

4 1

3’

41

42

43

c

61

62

63

64

65

Figure 7.2: Equivalent positions of a general atom through the symmetry operations associated to the various screw axes. We note that only axes 31 , 32 , 41 , 43 , 61 , 62 , 64 , 65 are chiral. We could therefore assume that the atoms equivalent through the symmetry operations associated to a screw axis form a chiral ﬁgure. But we must consider all the atoms equivalent within the unit cell, i.e. perform the operation modulo c. As a result, the ﬁgure obtained is not always chiral, as Figure 7.2 shows. Consider for example the case of a 42 axis. The 42 operations performed successively on atom 1 lead to atom 2, then to atom 3, then to atom 4 rotated by 3π/2 and translated by 3c/2 with respect to atom 1. The atom equivalent to 4 through a lattice translation operation −c is atom 4. The transform of atom 4 is atom 5. The atom at 3 is the equivalent of atom 3 through translation −c. We see that the equivalent positions produced, within a unit cell, by these operations 42 do not form a helix or screw, and that the ﬁgure features

134

Symmetry and Physical Properties of Crystals

mirror symmetry. In the same way, the ﬁgures associated to axes 21 and 63 (i.e. axes qm where q = 2m) are not chiral. We note that, among the chiral ﬁgures, those associated to axes 31 , 41 , 61 and 62 are respectively symmetric through a mirror operation of the ﬁgures associated to axes 32 , 43 , 65 and 64 . These ﬁgures are said to be enantiomorphic of each other.

¯ Deﬁnition of glide mirrors 7.2.2. S is a rotoinversion, noted S. We proceed in the same way as for rotations, i.e. we ﬁrst look whether a change in position of the rotoinversion axis makes it possible to reduce the translation to zero. Equation (7.1) is ¯ OO = t (E − S)

(7.4)

which we now solve, not geometrically as was done for rotations, but through ¯ is a rotation S followed by matrix algebra. We recall that rotoinversion S ¯ inversion, S = IS. We choose a system of axes Oxyz such that axis Oz coincides with the rotation axis, and O is the inversion center. In this axis system: ⎛ ⎞ − cos ϕ sin ϕ 0 0⎠ , S¯ = IS = ⎝ − sin ϕ − cos ϕ 0 0 −1 ⎛ ⎞ 1 + cos ϕ − sin ϕ 0 E − S¯ = ⎝ sin ϕ 1 + cos ϕ 0 ⎠ . 0 0 2 In order for Equation (7.4) to have a solution for all t, the determinant of ¯ det(E − S), ¯ must be non-zero. E − S, ¯ = 2(1 + cos ϕ)2 + 2 sin2 ϕ = 2(2 + 2 cos ϕ) = 8 cos2 ϕ/2. det(E − S) This determinant is zero if ϕ = π, i.e. only for a ¯2 axis. In all other cases, Equation (7.4) has a solution, and zero translation can be obtained through a change in origin. Let us therefore consider the operations associated to a ¯2 axis. We recall that a ¯ 2 axis is equivalent to a mirror perpendicular to it, which goes through the inversion center used for the rotoinversion. The rotation angle ϕ is equal ⎛ 0 ⎝ 0 0

to π, and Equation (7.4) becomes: ⎞ 0 0 0 0 ⎠ OO = t. 0 2

This equation has a solution only if t is parallel to axis Oz, the rotoinversion axis, and therefore perpendicular to the mirror.

Chapter 7 – Space groups

135

Let us note this translation t⊥ , and the associated symmetry operation (m, t⊥ ). In this case OO = t⊥ /2. We deduce the following result (Exercise 4.1): The product of a mirror operation and a translation t⊥ , perpendicular to this mirror, is equivalent to a mirror operation without translation provided the mirror is translated by t⊥ /2. The mirror operations which cannot transform into (m, 0) (pure mirrors) through displacement of the mirror are therefore of the form (m, t// ) where t// is parallel to the mirror. We calculate the product of this mirror operation by itself, using Equation (7.3). (m, t// )2 = (m, t// )(m, t// ) = (E, m t// + t// )= (E, 2t// ) which must be a symmetry operation of the crystal, and more precisely a lattice translation since the rotation part is the identity operation. Therefore 2t// must be a crystal lattice vector. We choose in the mirror plane two elementary lattice translations, which we note as a and b. We must have 2t// = ua + vb with u and v integers: u v (7.5) t// = a + b. 2 2 Since the required translations t// are deﬁned modulo the lattice translations, the solutions are restricted to the following cases: (a) t// = a/2 (u = 1 and v = 0): the mirror is called an axial mirror and noted as a, (b) t// = b/2 : the mirror, called axial, is noted b, (c) t// = a/2 + b/2 (u = 1 et v = 1) : the mirror, called diagonal is noted n, (d) t// = 0 : the mirrors without translation, or pure mirrors, are noted m. We chose to call a and b the basis vectors parallel to the mirror, i.e. to consider a mirror parallel to the (a, b) plane. Clearly, the mirror can be parallel to the (a, c) plane, with a translation a/2 (a-type mirror) or c/2 (c mirror), or a/2 + c/2 (n mirror). It can also be parallel to the (b, c) plane with a translation b/2 (b mirror) or c/2 (c mirror) or b/2 + c/2 (n mirror). Tables 7.2 and 7.3 show the symbols used to represent these various mirrors, for two orientations of the projection plane: perpendicular to the mirror for Table 7.2, and parallel to the mirror for Table 7.3. In order to keep the presentation simple, we assumed that the projection plane is parallel to a and b and that, in the case of a monoclinic lattice, c is the basis vector perpendicular to the two others. When the unit cells are multiple, we must also take into account the vector, or vectors, describing the lattice mode, which we note as T . For example,

136

Symmetry and Physical Properties of Crystals Table 7.2: Representation of mirrors perpendicular to the projection plane (a, b)

Nature of the mirror Notation Graphical representation Pure mirror

Translation

m

none

a, b

1/2 along the projection

c

1/2 perpendicular to the projection plane

n

1/2 along the projection + 1/2 perpendicular to the projection plane

Axial mirror

Diagonal translation mirror

Table 7.3: plane (a, b)

Representation of mirrors parallel to the projection

Nature of the mirror Notation Graphical representation

Translation

Pure mirror

m

none

Axial mirror

a, b

1/2 along the arrow

n

1/2 along the arrow

Diagonal translation mirror

for an I lattice, the vector 12 (a + b + c) and, for an F lattice, the three vectors 12 (b + c), 12 (c + a) and 12 (a + b) which complement the (integral) translations ua + vb + wc. Mirrors parallel to these lattice mode vectors, with a glide equal to T /2, are then possible. These mirrors are called diamond mirrors, because they exist in the diamond structure, introduced in Section 7.5.3. Their symbol is d.

7.2.3. Product of a symmetry operation and a translation We return to the cases where a change of origin can change an operation (S(O), t) into (S(O ), 0), whether S is a rotation or a rotoinversion, in order to ﬁnd the rules for performing this change in origin easily. We thus investigate successively the product of a rotation and a translation perpendicular to the rotation axis, of a mirror symmetry and a translation perpendicular to the mirror, and of a rotoinversion and any translation. In all these cases, the result of the product with the translation is just a displacement of the symmetry element implied (rotation axis, mirror or rotoinversion axis).

Chapter 7 – Space groups

137

Product of a rotation and a translation perpendicular to the rotation axis Consider a symmetry operation (S, t⊥ ) where S is a rotation by ϕ = 2π/n about an axis An going through point O, and t⊥ is a translation perpendicular to this axis. Condition (7.2) can be represented geometrically in the plane perpendicular to the rotation axis going through O (Fig. 7.3). We can search for O in this plane, since the position of the origin of rotations along an axis is arbitrary. Let OO be the transform of OO through rotation S. Condition (7.2) shows that O O must be equal to t⊥ . The ﬁgure shows a vector OP equal to O O , hence to t⊥ , as well as parallelogram OPO O . We see that the required point O is the apex of an isosceles triangle with the vector t⊥ drawn from O for its base, and with the rotation angle ϕ for its apical angle. We can thus state the following rule: Operation [S(O), t⊥ ] where S(O) is a rotation by ϕ around an axis going through O, and t⊥ a translation perpendicular to the axis, is equivalent to the pure rotation [S(O ), 0] if point O is on the perpendicular bisector of the segment t⊥ drawn from O and if, from this point, vector t⊥ subtends angle ϕ. O”

t

O

O’

t

P

Figure 7.3: Schematic diagram illustrating Equation (7.2). The new axis of rotation is located at O , on the bissector of OP = t⊥ . Here are two examples of applications. 1.

Consider a crystal with an orthorhombic unit cell, with 2-fold axes parallel to the basis vector c, and choose the origin of the unit cell on one of these 2-fold axes. Figure 7.4a is a projection of the orthorhombic unit cell onto a plane perpendicular to c. Because the crystal is periodic, there is also a 2-fold axis at the other apices of the unit cell. Consider operation [S(O), a], the product of operation S, a rotation by π around the 2-fold axis going through point O, and the lattice translation a perpendicular to the axis. This symmetry operation is equivalent to an operation [S(O ), 0]. According to the above rule, O lies on the perpendicular bisector of segment OA = a, and the angle which OA subtends from O is π. O is therefore the middle of segment OA (Fig. 7.4a). In the same way, performing the product of this rotation by π around the axis going through O and of the translation a + b (or b), we obtain a 2-fold axis located at the center S of rectangle OABC (or at O such that OO = b/2), etc. The set of 2-fold axes present in the unit cell are shown on Figure 7.4b.

2.

Consider a crystal with a tetragonal unit cell featuring 4-fold axes parallel to basis vector c. Figure 7.4c is the projection of this unit cell onto a

138

Symmetry and Physical Properties of Crystals plane perpendicular to c. Let S be the operation rotation by π/2 around the 4-fold axis parallel to c and going through O. Operation [S(O), a] is equivalent to [S(O ), 0] if O is at the center of unit cell OABC because segment OA subtends an angle π/2 from O . Further, a 4-fold axis contains a 2-fold axis which, when combined with the lattice translations, leads to the existence of the 2-fold axes represented on Figure 7.4c. O O’ a

O”

b

C

b

O /2

S

C

O’

a

A

B

(a)

A

(b)

B

(c)

Figure 7.4: (a) Primitive orthorhombic unit cell featuring a 2-fold axis at each lattice node; (b) set of 2-fold axes obtained through the composition of the symmetry operations around these axes with the lattice translations; (c) set of symmetry operations of a tetragonal unit cell of a lattice featuring a 4-fold axis at each lattice node Product of a mirror operation and a translation perpendicular to the mirror The symmetry operation (m, t⊥ ) resulting from the combination of a mirror operation and a translation t⊥ perpendicular to it is equivalent to (m, 0) if the mirror is translated by t⊥ /2. This rule, derived in Section 7.2.2 and in Exercise 4.1, and the previous one, are widely used to determine all the symmetry operations present in a unit cell starting from the generating elements of the space group and the lattice translations. Product of a rotoinversion and a translation We give the results without derivation in order not to make the text too long. The operation product of an inversion (equivalent to a 1¯ axis) and a translation t is equivalent to an inversion without translation if the center is translated by t/2. To determine the change in origin which makes it possible to cancel the trans¯ t) where S ¯ is a rotoinversion associated to a ¯3, ¯4, lation in an operation (S, or ¯6 axis, the translation must be decomposed into its t// and t⊥ components, respectively parallel and perpendicular to the axis. Component t⊥ is canceled by an operation similar to that of Section 7.2.3: point O is replaced by point O located in the plane perpendicular to the axis which goes through O and on the perpendicular bisector of segment OP = t⊥ , such that, from O , OP subtends the angle ϕ − π. Component t// is canceled by submitting O to ¯ ¯ ), 0]. t] = [S(O translation O O = t// /2. We thus obtain [S(O),

Chapter 7 – Space groups

139

7.3. Enumeration of space groups Starting from a given point group G0 G0 = (E, 0) + (S1 , 0) + (S2 , 0) + (S3 , 0) + . . . + (Sm , 0), we want to determine the various space groups Gs which are associated to it, and which can be written as: Gs = (E, 0) + (S1 , t1 ) + (S2 , t2 ) + (S3 , t3 ) + . . . + (Sm , tm ) (modulo T), taking into account the fact that the operations (Si , ti ), where ti is nonzero, are associated to screw axes or to glide mirrors. We recall that all the operations (Si , ti ) here have a common origin. This determination can be performed systematically for all the point groups, starting from the simplest ones and using a few theorems deduced from the isomorphism between the quotient group G/T and the point group G0 to which it is associated. This procedure is tedious, and we will just illustrate the method through an example, that of the space groups deduced from point group mm2. Point group mm2, associated to an orthorhombic unit cell with basis vectors a, b and c, contains the following symmetry operations: rotation by π around an axis which we can assume to be parallel to c for example, and which we note (A, 0), symmetry with respect to a mirror perpendicular to a, which we call (m1 , 0), symmetry with respect to a mirror perpendicular to b, which we note (m2 , 0), and identity (E, 0). G0 = (E, 0) + (A, 0) + (m1 , 0) + (m2 , 0). The mirrors intersect along the 2-fold axis, here parallel to c.

7.3.1. Symmorphic space groups The ﬁrst space group that comes to mind is group Gs , associated directly to point group G0 : Gs = (E, 0) + (A, 0) + (m1 , 0) + (m2 , 0) (modulo T). This means that all the symmetry operations of the crystal are the four operations forming G0 and all their products with lattice translations n = ua +vb + wc. We now choose an axis system Oxyz, parallel to a, b, and c respectively, and take for a unit, along each of these axes, the length of the respective lattice parameter, a, b or c. If an atom in the unit cell has coordinates x, y, z, the presence of the symmetry elements implies the existence of an atom of the same

140

Symmetry and Physical Properties of Crystals

kind at points with coordinates −x, −y, z (operation A, 0), −x, y, z (operation m1 , 0) and x, −y, z (operation m2 , 0). Additionally, there are of course all the positions deduced from the above through the lattice translations, but this goes without saying. Thus the “equivalent positions” of an atom in a general position are deﬁned. The coordinates of these positions are: (x, y, z)

(−x, −y, z)

(−x, y, z)

(x, −y, z).

The space group is noted as Pmm2, with P saying that the lattice is primitive. Consider the cases where the orthorhombic unit cell is a multiple cell. We know it can be base-centered (A, B or C lattice), body-centered (I lattice) or face-centered (F lattice). (a) Body-centered lattice. The crystal lattice features, apart from the translations n = ua + vb + wc which form group T, a lattice mode translation T with coordinates ( 12 , 12 , 12 ). The corresponding space group will be deﬁned by the set of the above operations and of those deduced from them through translation T , so that the new space group is: Gs = (E, 0) + (A, 0) + (m1 , 0) + (m2 , 0) + (E, T ) + (A, T ) + (m1 , T ) + (m2 , T ) (modulo T). The coordinates of equivalent positions are now: (x, y, z)

(x + 1/2, y + 1/2, z + 1/2)

(−x, −y, z)

(−x + 1/2, −y + 1/2, z + 1/2)

(−x, y, z)

(−x + 1/2, y + 1/2, z + 1/2)

(x, −y, z)

(x + 1/2, −y + 1/2, z + 1/2).

This new space group is called Imm2.

(b) Base-centered lattice. For example, in the A lattice, translation T 0, 12 , 12 is added, and the corresponding space group is noted Amm2. The coordinates of equivalent positions will now be: (x, y, z)

(x, y + 1/2, z + 1/2)

(−x, −y, z)

(−x, −y + 1/2, z + 1/2)

(−x, y, z)

(−x, y + 1/2, z + 1/2)

(x, −y, z)

(x, −y + 1/2, z + 1/2).

(c) Face-centered lattice. The F lattice adds translations T 1 0, 12 , 12 , T 2 ( 12 , 0, 12 ), T 3 12 , 12 , 0 . The space group for the F lattice, noted Fmm2, is thus: Gs = (E, 0) + (A, 0) + (m1 , 0) + (m2 , 0) + (E, T 1 ) + (A, T 1 ) + (m1 , T 1 ) + (m2 , T 1 ) + (E, T 2 ) + (A, T 2 ) + (m1 , T 2 ) + (m2 , T 2 ) + (E, T 3 ) + (A, T 3 ) + (m1 , T 3 ) + (m2 , T 3 ) (modulo T)

Chapter 7 – Space groups

141

and the equivalent positions are: (x, y + 1/2, z + 1/2)

(x, y, z)

(−x, −y, z) (−x, −y + 1/2, z + 1/2) (−x, y, z)

(−x, y + 1/2, z + 1/2)

(x, −y, z)

(x, −y + 1/2, z + 1/2)

(x + 1/2, y, z + 1/2)

(x + 1/2, y + 1/2, z)

(−x+ 1/2, −y, z+ 1/2) (−x+ 1/2, −y+ 1/2, z) (−x + 1/2, y, z + 1/2)

(−x + 1/2, y + 1/2, z)

(x + 1/2, −y, z + 1/2)

(x + 1/2, −y + 1/2, z).

This provides the enumeration of the so-called symmorphic space groups, which are the space groups where all the symmetry operations are of the form (S, 0) modulo the lattice translations T for the primitive unit cells, or (S, 0) and (S, T ) modulo T for the multiple unit cells. The number of these space groups for a given crystal system is equal to the number of point groups multiplied by the number of Bravais lattices. We thus obtain a total of 66 symmorphic space groups (Tab. 7.4). Their notation includes a letter which deﬁnes the lattice, followed by the symbol for the point group. Table 7.4: Enumeration of the 66 symmorphic groups, to which 7 supplementary groups must be added

System

Number of point groups

Number of Bravais lattices

Number of space groups

Triclinic

2

1

2

Monoclinic

3

2

6

Orthorhombic

3

4

12

Tetragonal

7

2

14

Rhombohedral

5

1

5

7+5

1

12

5

3

15

Hexagonal Cubic

Seven other groups must be added to these 66 groups, for two diﬀerent reasons. On the one hand, there can be various ways of associating the Bravais lattice translation T to a given point group. This is the case for the basecentered orthorhombic groups, associated to point group mm2, for which it is

142

Symmetry and Physical Properties of Crystals

not equivalent to center the bases parallel or perpendicular to the 2-fold axis: this yields groups Amm2 and Cmm2. On the other hand, there can also be two diﬀerent ways of positioning the symmetry elements with respect to the elementary lattice translations. For example, crystals with point group ¯42m can have their basis vectors parallel either to the mirrors or to the 2-fold axes, and this results in the existence of two diﬀerent space groups, P¯42m and P¯4m2 (the notations are explained in Sect. 7.4). For the same reason, there exist I¯42m and I¯4m2, P312 and P321, P3m1 and P31m, P¯3m1 and P¯31m, P¯6m2 and P¯62m (Exercise 7.1). We thus obtain the 7 supplementary groups (one for the ﬁrst reason, and 6 for the second reason).

7.3.2. Non-symmorphic space groups We again consider point group mm2: G0 = (E, 0) + (A, 0) + (m1 , 0) + (m2 , 0). Primitive groups We replace one or more of the (S, 0) symmetry operations by compatible operations (S, ti ), where the ti are non-zero, i.e. by the operations associated with screw axes or glide mirrors. We ﬁrst replace the pure mirror m2 , perpendicular to basis vector b, by a glide mirror. Symmetry operation (m2 , 0) is thus successively replaced by the symmetry operations (m2 , a/2), (m2 , c/2) and (m2 , a/2+c/2) while retaining (m1 , 0). The symmetry operations have a common origin, chosen on the 2-fold axis where mirrors m1 and m2 intersect. 1.

The group contains, instead of (m2 , 0), operation (m2 , a/2) associated to an a-type mirror. It also contains, by assumption, (m1 , 0), and therefore the product (m2 , a/2)(m1 , 0), calculated using Equation (7.3). This product is equal to (A, a/2), where the 2-fold axis goes through the common origin O. Since translation a/2 is perpendicular to the 2-fold axis, a change in the position of this axis leads to zero translation. Applying the rule of Section 7.2.3 shows that the new axis goes through point O such that OO = a/4 (Fig. 7.5a), since segment OP = a/2 subtends angle π from O . The space group is Gs = (E, 0) + (m1 , 0) + (m2 , a/2) + (A, 0)

(modulo T)

(7.6)

where the indicated operations now do not all have the same origin. Relation (7.6) must be used in connection with Figure 7.5b, which shows the respective positions of the symmetry elements. This group is called Pma2 (group 28 in I.T. A) because we will see, in Section 7.4, that the notation of the space groups in the orthorhombic system is based on the following order for the symmetry elements: ﬁrst the mirror

Chapter 7 – Space groups b

O

m1 O’

a

143

O

C

O’

P A m2

B

(a)

(b)

(c)

(d)

(e)

(f)

Figure 7.5: An example of the determination of space groups deduced from point group mm2. Operation (m2 , 0) is successively replaced by (m2 , a/2), leading to group Pma2 ((a) and (b)), then by (m2 , c/2), leading to space group Pmc21 ((c) and (d)), and ﬁnally by (m2 , a/2 + c/2), leading to space group Pmn21 ((e) and (f)). perpendicular (or the axis parallel) to a, then the mirror perpendicular (or the axis parallel) to b, then the same for c. Figure 7.5b shows the corresponding unit cell OABC, with all the symmetry elements in the unit cell indicated. They are determined by applying the rules of Section 7.2.3 to the products of the operations m1 , m2 and A with the lattice translations. For example the product of (m1 , 0) and the lattice translation a perpendicular to m1 is equivalent to a pure mirror translated by a/2 (rule in Sect. 7.2.3). In the same way, the product of (m2 , a/2) and the lattice translation b perpendicular to m2 yields the same glide mirror translated by b/2. Applying the rule of Section 7.2.3 shows that the combination of the 2-fold axis going through O with a lattice translation n perpendicular to it (here a or b or (a + b)) is equivalent to the existence of a 2-fold axis translated by n/2. Thus there are 2-fold axes going through the points deduced from O through translations a/2, b/2 and (a + b)/2.

144 2.

Symmetry and Physical Properties of Crystals The group contains, instead of (m2 , 0), operation (m2 , c/2) associated to a c mirror. The product (m2 , c/2) (m1 , 0) is equal to (A, c/2), i.e. to a screw axis 21 at the intersection of the mirrors (Fig. 7.5c) and Gs = (E, 0) + (m1 , 0) + (m2 , c/2) + (A, c/2) (modulo T). The space group is noted Pmc21 (group 26, I.T. A) and Figure 7.5d shows all the symmetry elements present in the unit cell.

3.

The group contains, instead of (m2 , 0), operation (m2 , a/2 + c/2) associated with an n mirror. The product operation (m2 , a/2 + c/2)(m1 , 0) is equal to (A, a/2 + c/2), which can be replaced by operation (A, c/2) if the origin of the 2-fold axis is displaced by a/4 (Fig. 7.5e). The space group is Gs = (E, 0) + (m1 , 0) + (m2 , a/2 + c/2) + (A, c/2) (modulo T). It is noted Pmn21 (group n◦ 31, I.T. A) and Figure 7.5f shows all the symmetry elements present in the unit cell.

Other space groups are obtained by substituting glide mirrors for the two mirrors: for example (m1 , b/2) and (m2 , a/2). The product of these two operations is equal to (A, −a/2+b/2), which becomes (A, 0) if the rotation axis is submitted to translation −a/4 + b/4. The group is noted Pba2 (group 32, I.T. A). In the same way, the reader can, as an exercise, consider the various possible combinations of glide mirrors (Exercise 7.3 is an example). This will show that the combination of operations: (m1 , c/2) and (m2 , a/2) leads to group Pca21 (group 29, I.T. A), (m1 , b/2 + c/2) and (m2 , a/2) leads to group Pna21 (group 33, I.T. A), (m1 , c/2) and (m2 , c/2) leads to group Pcc2 (group 27, I.T. A), (m1 , b/2 + c/2) and (m2 , c/2) leads to group Pnc2 (group 30, I.T. A), (m1 , b/2 + c/2) and (m2 , a/2 + c/2) leads to group Pnn2 (group 34, I.T. A). We thus enumerated a total of 10 primitive groups associated to point group mm2. Characterizing each of them involves a schematic drawing indicating the position of the various symmetry elements present in the unit cell. Non-primitive groups The non-primitive space groups can be enumerated starting from each of these 10 primitive groups, by adding the lattice mode translation or translations T , which transform(s) them into a non-primitive lattice. However, the combination of a glide mirror and a translation T can yield a pure mirror translated with respect to the ﬁrst one if translation T contains a component, parallel to the mirror, equal to the glide vector.

Chapter 7 – Space groups

145

Thus consider group Pma2, the symmetry elements of which are represented on Figures 7.5b and 7.6a. In Figure 7.6a, the origin of the unit cell is chosen on a 2-fold axis to conform to the International Tables for Crystallography A (Sect. 7.3.3). Suppose the group is now C-type, meaning that base (a, b) is centered, which adds the lattice translation T = 12 (a + b). The symmetry operation corresponding to this translation is noted ST = (E, 1/2 [a + b]) . The new space group includes the operations of Gs given in Equation (7.6), which must be associated to Figure 7.6a, and the result of combining them with ST . We investigate them in turn. b

a

(a)

(b)

(c)

Figure 7.6: Symmetry elements present in the unit cells of (a) group Pma2; (b) group Pma2 with the (a, b) faces centered, becoming Cmm2; (c) group Cmm2 when the origin is placed on an intersection of two pure mirrors as in I.T. A The composition of (m2 , a/2) with ST is obtained by using relation (7.3), where the rotation or rotoinversion operations are taken to have the same origin. (E, 1/2 [a + b]) (m2 , a/2) = (m2 , [a + b/2]) = (m2 , b/2)

(7.7)

modulo T.

We ﬁnally obtain a glide mirror operation, with a translation b/2 perpendicular to the mirror. It transforms into a pure mirror operation by translating the mirror by b/4 (Fig. 7.6b). Relation (7.7) leads to the remark that combination with a pure translation simply adds this translation to the original translation part. The composition of (m1 , 0) with ST gives (m1 , a/2 + b/2). The translation part has two components: a/2, perpendicular to the mirror, which can be canceled by translating the mirror by a/4, and b/2, parallel to the mirror, which turns it into a glide mirror. Combining (A, 0) with ST displaces the 2-fold axis by 14 (a + b). All the symmetry elements present in the unit cell are represented on Figure 7.6b. We see that there are pure mirrors perpendicular to a and b. The space group is Cmm2. Figure 7.6c shows the unit cell, taking for the origin the intersection of mirrors as in volume A of the International Tables for Crystallography.

146

Symmetry and Physical Properties of Crystals

In contrast, if a lattice translation T = 12 (b + c) is added to group Pma2, the lattice becomes base-centered A, and we obtain group Ama2, the symmetry elements of which are shown on Figure 7.7. b

a

Figure 7.7: Symmetry elements of space group Ama2 The non-primitive space groups associated to point group mm2 are thus fewer than the primitive groups. In International Tables A, the following groups are found: Cmm2, Cmc21 , Ccc2, Amm2, Abm2, Ama2, Aba2, and Fmm2. The aim of this section was to show one procedure for the enumeration of space groups. Their complete enumeration is beyond the scope of this book. There are 230 crystallographic space groups, perfectly described in volume A of International Tables for Crystallography, which is presented in the following section.

7.3.3. International Tables for Crystallography The 230 space groups are cataloged in volume A of the International Tables for Crystallography (I.T. A) which, for each group, provide lots of information, as shown on the two pages reproduced on Figures 7.8 a and b, dedicated to space group P4/n, numbered 85. The ﬁrst of theses pages is reproduced on Figure 7.8a. The ﬁrst line indicates the name of the space group in the Hermann-Mauguin 3 ), then the associated notation (P4/n), then in the Schönﬂies notation (C4h point group (4/m), and ﬁnally the associated crystal lattice (tetragonal). Since the lattice is primitive, the orders of the space group and the point group are equal, in this case to 8. The 8 symmetry operations of the space group are listed under “Symmetry operations”, where each operation is numbered and its nature and position described. For example operation (6), noted n 12 , 12 , 0 x, y, 0, is the symmetry operation “mirror with diagonal translation n”, the glide component of which is the vector 12 , 12 , 0 , with the position of the mirror being given by its equation z = 0 or (x, y, 0). The left-hand ﬁgure is the projection onto a plane perpendicular to the highestorder axis (here the 4-fold axis) of all the symmetry elements present in the unit cell. The basis vectors a and b are oriented as on the earlier ﬁgures (7.5 to 7.7). The symbols used for this representation were introduced in Tables 7.1 to 7.3.

Chapter 7 – Space groups

147

Figure 7.8a: Reproduction of a page of volume A of the International Tables for Crystallography: ﬁrst page describing group P4/n (© IUCr, with permission) The origin of the chosen unit cell is indicated under the ﬁgures. Here it is taken on the center of inversion for the ¯4 axis, and this is the ﬁrst choice of the International Tables A. For this group, the Tables also oﬀer another version, not reproduced here, where the origin of the unit cell is chosen on a center of symmetry. The right-hand ﬁgure indicates the general positions of the atoms, the signs + and − standing for coordinates + z and − z respectively. The circles with a comma are the images of the circles without comma through one of the improper symmetry operations of the group (mirror, inversion or rotoinversion). Page 2 (Fig. 7.8b) ﬁrst presents a choice of generating elements for the space group, then the various possible positions for an atom (indexed through a letter, called the Wyckoﬀ symbol), starting with the general position, for which the coordinates x, y, z are general. The following positions are special positions, because they are located on one or several symmetry elements. For each position, the table gives the coordinates of the equivalent positions (modulo the lattice translations) through the symmetry operations of the group. For the general position, the atoms in positions equivalent through the symmetry operations are numbered from (1) to (n) where n is the order of the group.

148

Symmetry and Physical Properties of Crystals

Figure 7.8b: Reproduction of a page of volume A of the International Tables for Crystallography: the second page describing group P4/n (© IUCr, with permission) The atom in position (k) deduces from atom in position (1) through the symmetry operation indexed as (k) on the ﬁrst page. For example, in the space group P4/n described, atom (3) deduces from atom (1) through operation (3), a rotation by π/2 around the 4-fold axis which goes through the point with coordinates x = 0, y = 12 . For each position, the table starts out by indicating its multiplicity (number of equivalent positions), then its Wyckoﬀ symbol (a letter given in alphabetical order, starting with the last position, the one with lowest multiplicity), then the local symmetry of this particular site, and ﬁnally the coordinates of the equivalent atomic positions. The local symmetry of a site in a special position deduces from the symmetry elements going through the site. The set of the symmetry operations associated to these symmetry elements which intersect

Chapter 7 – Space groups

149

on the site form a point group which is a subgroup of the point group of the crystal. The asymmetric unit, indicated on page 1, is deﬁned in a general way as a part of space such that, if it is submitted to all the symmetry elements of the space group, all of space is occupied. It is therefore bounded by planes. However, for a given crystal structure, the asymmetric unit is deﬁned by a group of atoms such that, when complemented by their images through all the symmetry operations of the space group, the motif (or pattern) of the crystal unit cell is retrieved. We note that the set of atoms in the motif of a crystal correspond to a multiple of the chemical formula of the material, while this is not necessarily the case for the atoms in the asymmetric unit. For example, the motif of the unit cell of quartz (chemical formula SiO2 , space group P31 21) contains three SiO2 groups, while the asymmetric unit consists of one Si atom and one O atom. Since the oxygen atom is in a general position with multiplicity 6, there are 6 oxygen atoms in the motif while the Si atoms are in a special position (on a 2-fold axis) with multiplicity 6/2 = 3, hence 3 silicon atoms in the motif. Starting with one Si atom and one O atom, we retrieve the set Si3 O6 , i.e. a motif of three SiO2 groups.

7.4. Nomenclature The Hermann-Mauguin space group notation starts with a letter indicating the nature of the Bravais lattice (P for primitive, A, B or C for base-centered, I for body-centered, and F for face-centered). It then refers directly to the notation of the point group which is associated to it (the notation is given in Chap. 5), making explicit the nature of the axes and mirrors involved in the notation for the point group. For example, if an n-fold axis is a screw axis, we add to the n involved in the point group notation a subscript p indicating that the translation is a fraction p/n of the basis vector parallel to the axis (Tab. 7.1). If one of the mirrors is a glide mirror, the letter m is replaced by a, b, c or n depending on the nature of the translation (Tab. 7.2). When the notation for the point group includes several identical signs, or involves an ambiguity, the following rules are applied, with the understanding that the quoted directions deﬁne, when the subject is an axis, its direction, and, for a mirror, the direction perpendicular to it. Orthorhombic system: the order is a, b, c. Example: group Cmc21 . The unit cell has its (a, b) bases centered. The point group is mm2. There are pure mirrors perpendicular to a, glide mirrors (translation c/2) perpendicular to b, and screw axes parallel to c (translation c/2). Tetragonal system: the ﬁrst sign refers to the 4 or ¯4 axis, which is always parallel to c, the second to the directions a and b, equivalent to each other, and the third to the bisectors of these directions in the (a, b) plane.

150

Symmetry and Physical Properties of Crystals Example: P¯ 42m is a space group with a primitive unit cell, with point group ¯42m. The ¯4 axis is parallel to c, there are 2-fold axes parallel to a and b, and pure mirrors at 45◦ to a and b. In group P¯4m2, the mirrors are parallel to a and b and the 2-fold axes are at 45◦ to a and b (Exercise 7.1). Hexagonal system: the ﬁrst sign refers to the 6-fold axis, parallel to c, the second to the directions of vectors a and b, and the third to the directions perpendicular to a and b. Example: P63 cm is a space group with a primitive unit cell, with point group 6mm; the 6-fold axis, parallel to c, is a screw axis (translation c/2); there are glide mirrors (glide c/2) perpendicular to a and b and pure mirrors parallel to a and b (since they are perpendicular to the normals to a and b). We now understand, on the basis of these examples, the rationale for the redundancy in the notation for some point groups. For example, in point group 6mm, the notation 6m is suﬃcient as a descriptor, since the generating elements of the group are the 6-fold axis and a mirror which contains it: the presence of these two generators leads to the existence of 6 mirrors enclosing angles of 30◦ with one another. However, these mirrors form two distinct families with respect to the symmetry operations of the space group. This leads to the existence of two diﬀerent space groups, P63 mc and P63 cm. Special case of the hexagonal lattices with rhombohedral point group: we recall (Sect. 6.3.3) that a crystal with rhombohedral point group (3, ¯3, 32, 3m or ¯3m) can have a rhombohedral lattice (noted R) or a hexagonal lattice (noted P). The rule for the hexagonal lattices applies to those with a hexagonal lattice, but with a 1 inserted where there is no symmetry element. Example of the group P31 21: the unit cell is hexagonal, the point group is 32, the 3-fold axis, parallel to c, is a screw axis (translation c/3), the 2-fold axes are parallel to a and b, and there is no 2-fold axis perpendicular to a and b. In contrast, for group P31 12, the 2-fold axes are perpendicular to a and b. Cubic system: same order as for the point group, viz. directions of the cube sides, then directions of the major diagonals of the cube, then directions of the face diagonals. First example: Pn¯3: primitive unit cell, point group m¯3, glide mirrors perpendicular to the cube edges (translation 12 (b + c) for the mirror perpendicular to a), 3-fold axes parallel to the major diagonals of the cube, and center of symmetry. ¯ Second example: Fd¯3m: face-centered cubic unit cell, point group m3m, diamond mirrors (see Sect. 7.2.2) perpendicular to the cube sides (translation 14 (b + c) for the mirror perpendicular to a), 3-fold axes parallel to

Chapter 7 – Space groups

151

the major diagonals of the cube and center of symmetry, pure mirrors perpendicular to the face diagonals. This is the space group of diamond and silicon crystals (see Sect. 7.5.3).

7.5. Examples: space groups of some structures 7.5.1. TiO2 -type structure (rutile) This structure2 is represented in a perspective view on Figure 8.4b. The unit cell is tetragonal primitive. The positions of the atoms in the unit cell are: Ti atoms : 0, 0, 0 and 12 , 12 , 12 ; O atoms:

u, u, 0;

1 2

+ u,

1 2

− u, 12 ;

1 2

− u,

1 2

+ u, 12 ;

−u, −u, 0.

The projection onto plane (a, b), with the heights z indicated, of the atom positions in two neighboring unit cells is shown on Figure 7.9a. The Ti atoms are shown as full circles and the O atoms as empty circles. This evidences a 42 axis which projects at A, glide mirrors (n mirrors) perpendicular to the sides a and b, with glides respectively 12 (b + c) and 12 (a + c), and pure mirrors parallel to the diagonals of the square. There is also a mirror parallel to the plane of the ﬁgure at height 0 (and another one at height 12 ). The point group is thus 4/m mm and the space group is P 42 /m nm. Since the point group is centrosymmetric, so is the space group. A center of symmetry projecting at A, with height 0, is evidenced. Figure 7.9b shows the axes and mirrors perpendicular to the projection plane. The 42 axis contains a 2-fold axis, and the products of the symmetry operations associated to this 2-fold axis with the lattice translations produce 2-fold axes at the apices and at the center of square (a, b). The centers of symmetry, represented by empty circles as usual, are also shown. Figure 7.9c shows all the symmetry elements present in the unit cell; this ﬁgure is excerpted from International Tables volume A (group 136). We note that the asymmetric unit here consists of one Ti atom and just one O atom, while the motif, outlined in dotted lines on Figure 7.9a, contains two TiO2 groups. The order of the point group is 16. It is equal to that of the space group since the unit cell is primitive. There are therefore 16 equivalent atoms in general positions. The oxygen atom is in a special position, at the intersection of two pure mirrors, hence on a site with multiplicity 16/4 = 4 while the Ti atom is at the intersection of 3 pure mirrors, thus on a site with multiplicity 16/8 = 2. Many crystals have this structure. Examples are CoF2 , MnF2 , CrO2 , PbO2 . The values of a, c and u vary from compound to compound.

2. TiO2 also exists under two other forms: anatase (tetragonal, I4/a md) and brookite (orthorhombic, Pbca).

152

Symmetry and Physical Properties of Crystals 0

b 0

0 0

0 0

½

a

½

A

½ ½

½ 0

0

Ti O

A

½ 0

0

0 0

0

(a)

(b) ¼

– –1 : 0 4:¼

¼

¼

¼

– 1 –:0 4:¼

– –1 : 0 4:¼

¼

¼

¼

– 1 –:0 4:¼ ¼

(c)

Figure 7.9: Structure of TiO2 . (a) Projection of the atoms onto plane (a, b), with the heights (z-coordinate) indicated. The Ti atoms are full circles and the O atoms empty circles. The dotted line surrounds the atoms which form the crystal motif. (b) Projection onto the same plane of the axes and mirrors present in the unit cell which are perpendicular to the plane. (c) Projection of all the symmetry elements present in the unit cell. Reproduction of a ﬁgure from volume A of the International Tables for Crystallography (© IUCr, with permission).

7.5.2. Metals with close-packed hexagonal structure This is the case for example of Zn, Na, Be, Mg, Cr. In this structure, which will be described in Chapter 8, the unit cell is hexagonal, with an atom at each of its vertices and another atom at position ( 23 , 13 , 12 ) as shown on Figure 7.10a, a projection of the atomic positions onto the base plane (a, b) indicating their coordinate parallel to c. Several contiguous unit cells were drawn in order to make the determination of the symmetry elements in this structure easier. By looking at the atom positions, we ascertain the presence of a 63 axis projecting at point A, a pure mirror with trace MN and two other mirrors of the same family (enclosing 60◦ angles between one another) going through A. We also distinguish a glide mirror with translation c/2, with trace uu (and two other mirrors of the same family going through A). Further, the plane of the ﬁgure (as well as the plane parallel to it at height 12 ) is a symmetry plane, hence

Chapter 7 – Space groups

M

153

0

0

½

u a 0

center of symetry at height ¼

½

b A

0

0

0

b

0

u’

½

a

½ 0

0

N

(a)

(b)

¼

¼

¼ ¼

¼

¼ ¼

¼ ¼

¼ ¼

¼

¼

¼

¼

¼ ¼

¼

¼

¼ ¼

¼

¼

¼

¼

¼

¼

¼ ¼

¼ ¼

¼ ¼

¼ ¼

¼ ¼

¼ ¼

¼ ¼

(c)

Figure 7.10: Close-packed hexagonal structure: (a) projection of the atomic positions, with the heights indicated, of four adjacent unit cells onto a plane perpendicular to c; (b) projection of some of the symmetry elements present in the unit cell; (c) projection of all the symmetry elements present in the unit cell, reproduced from I.T. A (group 194). The origin of the unit cell is at a center of symmetry located on the 63 axis. a pure mirror. We deduce that the space group is P 63 /m mc (group 194 in I.T. A). The point group is 6/m mm, which has a center of symmetry. There is a center of symmetry at height 14 , which projects at A. Figure 7.10b shows a single unit cell and the symmetry elements we just determined. Figure 7.10c shows all the symmetry elements in the unit cell, as found in International Tables volume A. We note, however, that, in International Tables, the origin of the unit cell is located on a center of symmetry which, on Figure 7.10a, projects at A and has height 14 . This explains why the mirror, parallel to the plane of the ﬁgure, which was at height 0 (with another one at

154

Symmetry and Physical Properties of Crystals

height 12 ) on Figure 7.10b, is at height 14 on Figure 7.10c, while the center of symmetry is noted with no further indication on Figure 7.10c since it is in the projection plane.

7.5.3. Structure of diamond The structure of diamond is shown on Figure 8.6 in a perspective view. This is also the structure of silicon and germanium. The unit cell is face-centered cubic and the projection of the carbon atoms onto the plane perpendicular to one of the sides of the cubic cell, the (a, b) plane for example, is represented, with height indications, on Figure 7.11a. The motif (or pattern) consists of two atoms (surrounded by a dotted line), with coordinates respectively (0, 0, 0) and ( 14 , 14 , 14 ). This structure features 3-fold axes along the major diagonals of the cubic unit cell. 0

0

½ ¾

¼

b ½ ¼

0,½ ¼,¾

0

0

0,½

½

0,½

0,½

3⁄8

1⁄8

1⁄8

3⁄8

¾

½

0

a

(a)

(b)

(c)

Figure 7.11: Structure of diamond, with face-centered cubic unit cell: (a) projection of the atom positions, with the heights indicated, onto plane (a, b); (b) position of the symmetry axes parallel to c; (c) projection of the mirrors perpendicular to the (a, b) plane Figure 7.11b shows the projection onto the (a, b) plane of the positions of the symmetry axes perpendicular to this plane. They are 41 , 43 and ¯4 axes. For the ¯4 axes, the height of the point used for inversion is indicated. In order not to clutter the ﬁgure, they are shown only in the upper left quadrant, because the ﬁgure is identical in all four quadrants. In the same way, the position and height of the centers of symmetry are shown only in the upper right quadrant. Figure 7.11c shows the mirrors perpendicular to the plane of the ﬁgure. The mirrors parallel to the cube faces are the glide mirrors with translation 14 (a + c) or 14 (a − c) for the mirrors perpendicular to b, and with translation 14 (b + c) or 14 (b − c) for the mirrors perpendicular to a. The two possibilities are distinguished by an arrow indicating the direction of the component of the translation vector along the projection plane, assuming the component perpendicular to the projection plane is positive. For example, if the translation vector is 14 (a + c), the arrow will be in the direction of a; if it is 14 (a − c), the arrow will be along vector −a, since the sign of the translation vector can be changed: if the translation vector is v to go from atom A to

Chapter 7 – Space groups

155

atom B, it is −v to go from atom B to atom A. These glide mirrors, for which the translation vector is a quarter of a lattice vector deﬁned by vectors a, b and c but half of a lattice mode vector T characterizing a multiple unit cell, are called diamond mirrors and noted d (see Sect. 7.2.2). The diagonal mirrors, perpendicular to the face diagonals, are pure mirrors. According to the rules stated in Section 7.4 (the ﬁrst symbol shows the nature of the mirrors perpendicular to the cube sides, the second symbol indicates the 3- or ¯3-fold axis, and the last symbol indicates the nature of the diagonal mirrors), the space group of the diamond structure is noted Fd¯3m.

7.6. Exercises Exercise 7.1 1.

(a) Consider point group ¯42m. Using a stereographic projection onto a plane normal to the ¯4 axis, show that the generating elements of this group can be either the ¯4 axis and a mirror parallel to this axis, or the ¯4 axis and a 2-fold axis perpendicular to this axis. (b) A crystal with this point group has a tetragonal lattice. Comparing the stereographic projections of the point groups of this crystal and its lattice, show that the basis vectors a and b of this lattice can be parallel either to the 2-fold axes, or to the mirrors. This leads to space groups P¯42m and P¯4m2 respectively. Determine, for each of these space groups, the equivalent positions for the general position x, y, z, and all the symmetry elements in the unit cell. Note that the ¯4 axis is at the intersection of the mirrors, and that the 2-fold axes intersect this ¯4 axis. Choose as the origin of the unit cell the point common to the various symmetry elements.

2.

We consider a crystal with point group 3m, and with a hexagonal lattice. (a) By comparing the point group of the crystal and that of the lattice, show that the three mirrors can be either parallel or perpendicular to the basis vectors a and b. (b) Two diﬀerent space groups are thus deﬁned, P31m and P3m1. Display, through a projection onto a plane perpendicular to the 3-fold axis, all the symmetry elements in the unit cell. (c) Why does the same approach fail to apply if the lattice is rhombohedral (space group R3m)?

Exercise 7.2 1.

Consider space group P4. Indicate all the symmetry elements present in the unit cell through a projection onto a plane perpendicular to the 4-fold axis.

156 2.

Symmetry and Physical Properties of Crystals The space group I4 is obtained by adding translation 12 (a + b + c) to the symmetry operations of group P4. Indicate all the symmetry elements present in the unit cell using a projection onto a plane perpendicular to the 4-fold axis.

Exercise 7.3 Determine the primitive space group deriving from point group mm2 and containing operations (m1 , c/2) and (m2 , a/2) where m1 is the symmetry operation associated to mirror M1 , perpendicular to a, and m2 the one associated to mirror M2 , perpendicular to b. Give its notation and the arrangement of the symmetry elements in the unit cell.

Investigation of some structures The following exercises deal with some crystal structures in the following way. We give the crystal system of the compound, and the position of the atoms in the unit cell. You are asked to determine the corresponding space group. This approach provides a better understanding of the notion of space group, and it is thus well suited to this book. We must however realize that this is not the approach used by a scientist who wants to determine the structure of a given crystal. The researcher starts out from an experimental result: the X-ray diﬀraction diagram given by this crystal. The accurate investigation of this diagram provides information on the space group of the crystal before the positions of the atoms in the unit cell are known. Exercise 7.4: structure of neptunium (Np) Between 278◦ C and 570◦ C, the crystal lattice of neptunium is tetragonal and the Np atoms are at the following positions: 0, 0, 0

1 1 2, 2,

1 2,

0

0, u

0, 12 , u ¯

1.

Determine the Bravais lattice.

2.

What is the local symmetry of each of the Np atoms? Give the corresponding point group for each of the sites, and deduce the group of which these two point groups are subgroups. This yields the point group of the crystal.

3.

Determine the nature of all the symmetry elements which make it possible to determine the space group. Indicate the space group.

Exercise 7.5: structure of NiAs Nickel arsenide, NiAs, crystallizes in the hexagonal system and the atom positions are: Ni As

0, 0, 0 1 2 3, 3, u

and and

0, 0, 12 , 2 1 1 3, 3, u + 2.

Chapter 7 – Space groups

157

1.

Draw a diagram, with the heights speciﬁed, of the atomic positions projected onto the plane perpendicular to c.

2.

Determine the symmetry elements present in the unit cell, and deduce the space group of the crystal.

3.

What is the symmetry of the Ni and As sites?

Exercise 7.6: structure of FeOCl Iron oxychloride FeOCl crystallizes in the orthorhombic system, and the atom positions are: Fe

0, 12 , u

and

Cl O

0, 0, v 0, 0, v

and and

1 2, 1 2, 1 2,

0, −u 1 2, 1 2,

−v −v

1.

Determine the Bravais lattice.

2.

Draw a diagram of the projection of the atoms onto a plane perpendicular to c, with the heights speciﬁed.

3.

Determine the symmetry elements present in the unit cell and the space group of this crystal.

4.

Give the number of equivalent positions for the general position and the coordinates of these positions.

158

Symmetry and Physical Properties of Crystals

Complement 7C. Structure determination: outline Solving a crystal structure means determining on one hand the geometry of the unit cell, and on the other hand the contents of the unit cell. The geometry involves the lengths and relative orientations of the sides of the unit cell that adequately describes the crystal symmetry. The contents of the unit cell involves the nature of the various atoms or ions, their average positions, and their thermal oscillations. The overwhelming majority of crystal structure determination work is based on the diﬀraction (coherent elastic scattering) of radiation, chieﬂy X-rays but in some cases neutrons. The replication of the unit cell inherent in crystal periodicity then allows ﬁnding the geometric characteristics and contents of the unit cell, whereas this would not be possible for a single unit cell. As shown by Bragg’s law (Sect. 3.2.3), the useful radiations must have wavelength smaller than the interatomic distances, hence the predominant use of X-rays. Neutron and electron diﬀraction, as discussed in Complement 4C, are also used, but to a much lesser extent. The frequency associated for example with X-rays of wavelength 0.05 nm (0.5 Å) is ν = c/λ = 3 × 108 /5 × 10−11 = 6×1018 Hz – far above the tracking possibilities of any instrument. As a result, only the intensity of the X-rays, but never their amplitude and phase, can be detected. Two sets of information must be collected. On the one hand, the geometrical conditions for coherent elastic scattering (diﬀraction) to occur, and on the other hand the eﬃciency of diﬀraction under this condition. The most convenient description of the geometrical condition for an incident wave, with wave-vector k0 , to be diﬀracted into a wave with wave-vector k is that the diﬀerence in wave-vector k − k0 be equal to a reciprocal lattice vector h∗ of the crystal, as introduced in Section 3.2.1 k − k0 = h∗ = ha∗ + kb∗ + lc∗ with a∗ , b∗ and c∗ the basis vectors of the reciprocal lattice and h, k and l integers. The geometrical information thus consists in the orientations and norms of the reciprocal lattice (Sect. 3.2) vectors h∗ , which we recall are vectors in reciprocal (or wave-vector) space. Each of them is associated with a Bragg reﬂection hkl, another name for the coherent elastic diﬀraction process with scattering vector h∗ . Another approach to diﬀraction by crystals consists in noting that, as is the case for visible light, the diﬀraction pattern is the representation of the modulus squared of the diﬀracted amplitude. The latter is the Fourier transform of the quantity which describes the interaction with matter. In the X-ray case, this is the electronic density ρe (r), the number of electrons per unit volume. If the crystal is supposed to be perfectly periodic, the (spatial) Fourier transform is non-zero only for discrete values of the scattering vector k − k0 , just as the

Chapter 7 – Space groups

159

(temporal) Fourier transform of a sound wave (periodic in time) only includes the fundamental frequency and its harmonics. This leads to the reciprocal lattice nodes h∗ = ha∗ +kb∗ +lc∗ shown above and introduced in Section 3.2.1. Each node of the reciprocal lattice, i.e. each vector h∗ , is characterized quantitatively in terms of the integrated reﬂectivity of the Bragg reﬂection Rhkl , the ratio of the area under a curve of diﬀracted power Pd versus crystal angle (rocking curve) over the intensity incident on the crystal: this quantity is signiﬁcant because it is independent of the divergence of the incident beam (Fig. 7C.1). The expression is discussed, without derivation, in the text below, which can be skipped on ﬁrst reading. Slit

Detector

Pd

Source Io

I 2 B

Crystal

(a)

(b)

Figure 7C.1: (a) A rotating crystal diﬀraction measurement on a single crystal. The diﬀracted beam is collected by a detector set at angle 2θB with respect to the incident beam, with θB the Bragg angle. (b) The variation of the diﬀracted power P d with the angle of the crystal, Ω, is the rocking curve. The integral under this curve, scaled with the power P 0 of the incident beam, is the integrated reﬂectivity.

Integrated reﬂectivity for X-rays under the kinematical approximation. Structure factor, Lorentz and polarization factors, Debye-Waller factor The expression for the integrated reﬂectivity can be shown to be Rhkl = λ3 V LP |ρhkl |2 where λ is the wavelength of the radiation used, V the volume of the crystal, L is the Lorentz factor, which depends only on the scattering angle and on the diﬀraction technique used (it is tabulated for example in International Tables for Crystallography, volume C), and P is the polarization factor, which depends only on the scattering angle and on the polarization of the incident beam (it is also tabulated in International Tables for Crystallography, volume C). The central quantity ρhkl is the hkl Fourier component of the scattering length density for the probe used. In the X-ray case, where the scattering is due to the electrons, ρhkl = rc ρe,hkl where rc is the length characterizing diﬀraction by a

160

Symmetry and Physical Properties of Crystals

single free electron and is called the classical electron radius, rc = 2.8×10−15 m and ρe,hkl the Fourier coeﬃcient hkl of the electron density ρe (r) in the crystal. Alternatively, we can write ρe,hkl = Fhkl /Vc , where Fhkl is called the structure factor of the Bragg reﬂection used, and Vc the unit cell volume. It is convenient to include in the expression for the structure factor the eﬀect of thermal vibrations of the atoms or ions through the so-called Debye-Waller factor. Then the structure factor can be written as fj exp[i(hxj + kyj + lzj )] exp{−Wj } Fhkl = j

or Fhkl =

fj exp[i(h∗ · rj )] exp{−Wj }.

j

In this expression, the sum is over all the atoms, indexed by subscript j, in the unit cell; fj is the atomic scattering factor (a function of the norm ||h∗ || of the scattering vector, at least in the approximation where the electron density in the atom has spherical symmetry), rj is the average position vector of the atom; exp{−Wj } is the Debye-Waller factor describing the vibration eﬀect; it reduces the scattering more heavily for those atoms which vibrate strongly, as well as for large scattering vectors. It is important to note that the experimentally measured quantity Rhkl is directly related to |ρhkl |2 and not to ρhkl . If ρhkl could be directly measured, determining the structure would be a trivial matter, since the electron density ρe (r) could then be reconstructed from its Fourier components. Actually the phase information is missing, and this is known as the phase problem in crystallography. Elaborate strategies, the discussion of which is beyond the scope of this complement, have been developed to obviate this problem. Structure determination is a largely computer-automated process. It can be performed with single crystal samples or with powders, where the sample consists of many tiny crystals, oriented at random. Powder diﬀraction, aided by computer ﬁles containing the results from a vast number of phases, is also a valuable tool for material identiﬁcation in industry or geology. More and more elaborate structures, involving larger and larger unit cells and more and more atoms in the unit cell, are determined routinely. A special case is that of materials of biological interest, where both the challenge and the eﬀorts are big, and where outstanding results in terms of basic science as well as for applications in medicine are obtained.

Chapter 7 – Space groups

161

Further reading A. Authier, The Reciprocal Lattice, International Union of Crystallography, Teaching Pamphlets (1981) C.A Taylor, A Non-mathematical Introduction to X-ray Crystallography, International Union of Crystallography, Teaching Pamphlets (2001); http://www.iucr.org/ data/assets/pdf ﬁle/0008/3050/1.pdf J.P. Glusker, Elementary X-ray Diﬀraction for Biologists, International Union of Crystallography, Teaching Pamphlets (2001); http://www.iucr.org/ data/assets/pdf ﬁle/0008/14399/15.pdf J.P. Glusker, K.N. Trueblood, Crystal Structure Analysis: A Primer (Oxford University Press, 1985)

162

Symmetry and Physical Properties of Crystals

References [1] Th. Hahn (ed.), International Tables for Crystallography, vol. A, Spacegroup Symmetry, 5th edn. (Kluwer Academic Publishers, Dordrecht, 2005)

Chapter 8

Chemical bonds and crystal structures This chapter introduces the various types of chemical bonds, and discusses how the nature of the bonds gives an insight into some crystal structures.

8.1. Introduction The periodic structure of crystals was ﬁrst evidenced by X-ray diﬀraction. This technique makes it possible to accurately determine not only the triple periodicity of the atomic arrangement, i.e. the crystal lattice, but also the positions of the individual atoms in the crystal motif. One may ask whether we can explain why one atomic arrangement rather than another one is obtained. This cannot be done in a systematic way. However, some rules emerge, and make it possible in many cases, not actually to predict the crystal structure, but rather, as we will see, to interpret the structure once it is determined. A crystal exists due to the cohesion between atoms, i.e. thanks to the existence of interatomic forces. The crystal structure is determined by the balance between the various interatomic forces. In order to understand the rationale for the various crystal structures, we therefore must start out by investigating these forces, i.e. the nature of chemical bonding in crystals and the special properties of each of these forces. Whatever the nature of the forces, one general rule applies: the atoms arrange in the most compact (or close-packed) way possible consistent with their size and the special requirements due to the nature of the force. The distance between two atoms in a solid results from the balance between the attractive and repulsive forces between these two atoms. The physical nature of the attractive force depends on the solid. It can be electrostatic as in ionic solids, or it can be a covalent binding force, or a Van der Waals force, or. . . Its variation as a function of the distance between the two atoms depends on the nature of these forces. In contrast, the repulsive force, due to the electrostatic repulsion between electrons and to Pauli’s “exclusion principle”,

© Springer Science+Business Media Dordrecht 2014 C. Malgrange et al., Symmetry and Physical Properties of Crystals, DOI 10.1007/978-94-017-8993-6_8

163

164

Symmetry and Physical Properties of Crystals

Energy

which forbids two electrons from being in the same quantum state, may in all cases be approximated by a 1/r 11 or 1/r 12 or exp(−r/ρ) function, where ρ is a characteristic radius. For all types of chemical bonds, the total potential energy looks like the curve shown on Figure 8.1. It has a minimum for a value r0 of r which is the equilibrium position. Since the repulsive energy varies, in all cases, much faster than the attractive energy, its contribution to the total energy at equilibrium (r = r0 ), noted U (r0 ), is small with respect to the attractive energy Eatt (r0 ). We may therefore obtain a fair order of magnitude of the total energy at equilibrium by considering only the attractive energy.

Repulsive energy

0

U(r0) Eatt(r0) Attractive energy 0

1

2

3

4

5

6

r/r0

Figure 8.1: Potential energy between two atoms as a function of their distance, expressed in units of the equilibrium distance r 0 of these two atoms (thick line) In this chapter, we describe the main bonding forces. For each of them, we ﬁrst show the properties of the corresponding arrangements (such as a deﬁnite number of ﬁrst neighbors, or not; well-deﬁned bond directions, or not. . . ). Then we indicate the order of magnitude of the bonding energy. We recall that the bonding energy of two atoms forming a molecule is the diﬀerence in energy between the isolated atoms (i.e. when they are located at inﬁnite distance from each other) and the atoms gathered into a molecule. In a general way, the bonding energy, also called cohesive energy, of a group of atoms forming a molecule or forming a crystal is the diﬀerence in energy between these atoms when isolated and the atoms in the form of the molecule or crystal. Finally, we give for each bond type a few examples of simple structures involving this type of force. We will mostly restrict this description to crystals containing one or two types of atoms.

Chapter 8 – Chemical bonds and crystal structures

165

8.2. Ionic bonds 8.2.1. Nature and properties An ion is an atom which lost or gained electrons, so that its outermost electronic shell is complete. Its electronic structure is then usually that of a rare gas. Example: the Na+ and Cl− ions. Their electronic conﬁguration, together with that of the non-ionized atoms, is shown in Table 8.1. Table 8.1: and ions

Electronic conﬁguration of sodium and chlorine atoms

Electronic state → Element or ion

1s

2s

2p

3s

Na

2

2

6

1

Na+

2

2

6

Cl

2

2

6

2

5

Cl−

2

2

6

2

6

3p

Ionic crystals are made up of positive and negative ions, and the Coulomb interaction is dominant. Because the crystal is neutral, charge compensation must occur, on the smallest scale possible, which leads to an alternation of positive and negative ions. Each ion is attracted by its nearest neighbors and repelled by its second neighbors. X-ray diﬀraction allows to determine accurately not only the positions of the centers of the atoms and thus their distance, but also the distribution ρ(r) of the electronic charge density. The distribution obtained, for example along the axis connecting the Na+ and the Cl− ions, in a crystal of NaCl is shown on Figure 8.2b, deduced from Figure 8.2a. We see that ρ(r) practically goes to zero between the ions (the minimum is less than one thousandth of the maximum density at the center of the ions). This justiﬁes the approach below, where the electrostatic interaction between Na+ and Cl− is treated as that of +q and −q point charges (where q is the electron charge), localized at the center of the ions. In fact, the measurement shown on Figure 8.2 can be performed on many ionic crystals, which are diﬀerent combinations of ions. The results of these accurate measurements lead to the following rule: to a rather good approximation, each species can be described as a “hard sphere” (meaning that it does not deform when it comes to contact), with a well-deﬁned radius called the ionic radius.

166

Symmetry and Physical Properties of Crystals

Electron density [e– Å–3]

200

Cl − 150

100

Na+ 50

0 0

(a)

0.4

0.8

1.2

1.6

2

2.4

2.8

Distance [Å] (b)

Figure 8.2: Electron density in a crystal of NaCl in the (hk0) plane: (a) iso-electron-density curves, after G. Schoknecht [1] (reproduced by kind permission of Verlag der Zeitschrift für Naturforschung, Tübingen, Germany); (b) variation in the electron density along the line connecting a Na+ ion to its nearest neighbor Cl− , as deduced from (a). The distance between the Na+ and Cl− ions is 2.815 Å. The approximation involved in the determination of ionic radii has two origins: 1.

The minimum in electron density between the two ions is rather ﬂat, and there is therefore some freedom of choice in determining where either of the sphere ends.

2.

The bonds in the solids considered as ionic are not always purely ionic, which can lead to slight variations from one solid to another. The ﬁrst set of ionic radii were published by Goldschmidt et al. [2] and Pauling [3], and their values are slightly diﬀerent. Table 8.2 shows the values of some ionic radii as determined by Shannon and Prewitt [4]. They showed that the values of these ionic radii depend on the coordination number (the number of nearest neighbors) of these ions. The values indicated in the table are those for coordination number 6.

The consistency of these values can be tested by comparing, as in Table 8.3, the anion–cation distances derived from these values and the distances measured in crystals with the NaCl structure, where these ions have coordination 6. In Table 8.2, the ions on a given row have the same electronic conﬁguration (the same number Z of electrons) as the rare gas shown on the same row. The charge of the nucleus increases from left to right, and consequently the attraction by the nucleus increases, which explains that the ionic radius decreases. In a given column, the ions have the same charge and, from top to bottom,

Chapter 8 – Chemical bonds and crystal structures

167

the charge of the nucleus increases, which tends to bring the electrons closer to the center, but the increase in the number of electrons tends to increase the volume of the ion. Table 8.2: Values, in Å, of some ionic radii in crystals, after [4] Ionic charge

2–

1–

Rare gas

1+

2+

He (Z = 2)

Li 0.74

Be 0.35

3+

O 1.40

F 1.33

Ne (Z = 10)

Na 1.02

Mg 0.72

Al 0.53

S 1.84

Cl 1.81

A (Z = 18)

K 1.38

Ca 1.00

Sc 0.73

Se 1.98

Br 1.96

Kr (Z = 36)

Rb 1.49

Sr 1.16

Y 0.90

Te 2.21

I 2.20

Xe (Z = 54)

Cs 1.70

Ba 1.36

La 1.06

Table 8.3: Comparison of the values of the anion–cation distances calculated from Table 8.2 and measured by X-ray diﬀraction (these values are from [5]) Compound

Calculated Measured distance distance

LiF

2.07

2.01

LiCl

2.55

2.565

LiBr

2.70

2.75

LiI

2.94

3.00

NaF

2.35

2.31

NaCl

2.83

2.815

NaBr

2.98

2.985

NaI

3.22

3.215

KF

2.71

2.67

KCl

3.19

3.145

KBr

3.34

3.30

KI

3.58

3.53

168

Symmetry and Physical Properties of Crystals

The competition between these two eﬀects explains why the ionic radius increases relatively little with atomic number Z. From Li+ to Cs+ the number of electrons grows from 2 to 54, a 27-fold increase (i.e. 33 ) while the ionic radius is multiplied, not by 3, but only by 2.3. Note: the forces involved are central, and thus independent of the bond direction, so that the various bonds of a given atom have no preferred relative orientation. The consequence is that the number of bonds between an atom and its ﬁrst neighbors can have any value, but is restricted by steric eﬀects. The structure of ionic crystals is thus characterized by the alternation of positive and negative ions, maximum compacity consistent with the respective ionic radii.

8.2.2. Bonding energy Consider again the NaCl crystal, known to have a face-centered structure (Fig. 8.3b). The Coulomb interaction energy between two ions Na+ and Cl− located a distance r from each other is given by ECoul = −e2 /r where e2 = q 2 /4πε0 , q being the electron charge and ε0 the electrical permittivity of vacuum. The bonding energy of a Na+ ion in a NaCl crystal can be calculated using the actual environment of the ion. We see on Figure 8.3 that a Na+ ion + distance r0 (ﬁrst neighbors), by 12 is surrounded by 6 Cl− ions at a √ √ Na ions − (second neighbors) at distance r0 2, by 8 Cl ions at distance r0 3, etc. The total Coulomb energy of a Na+ ion is therefore:

8 e2 e2 12 ECoul = − 6 − √ + √ − . . . = −α r0 r0 2 3 where α is called the Madelung constant of NaCl. The series which must be summed to obtain α is an alternating, slowly converging series. Computing it accurately requires special approaches. For NaCl (and for any other face-centered cubic structure of the AX type, where the ions A and X are monovalent) the value of α is 1.748, so that ECoul = −1.748

e2 . r0

For other structures, other values of α are obtained. We note that the same result would be obtained by considering a Cl− ion and its neighbors. The value of r0 is obtained from the lattice parameter a determined by X-rays, viz. a = 5.63 Å for the cubic cell of NaCl and r0 = a/2 = 2.815 Å. The value deduced for ECoul is −8.92 eV, hence an attractive energy of 8.92 eV per ion. If we take into account the repulsive energy, we obtain 7.89 eV. The binding energy measured from the heat of sublimation is 7.86 eV, in very good agreement considering the simplicity of the model.

Chapter 8 – Chemical bonds and crystal structures

Cs+

Cl–

(a)

Na+

Cl–

(b)

169

Zn2+

S2–

(c)

Figure 8.3: Examples of structures of ionic crystals with formula AX: (a) cesium chloride CsCl, primitive cubic; (b) sodium chloride NaCl (rocksalt), fcc; (c) zinc sulﬁde ZnS, fcc. In each of these structures, the motif consists of one anion–cation neighbor couple.

8.2.3. Ionic structures with formula AX The simplest and most frequent of these are the CsCl, NaCl and ZnS-type structures, shown on Figure 8.3. The CsCl structure is primitive cubic (Fig. 8.3a). The motif consists of a Cs+ ion and a Cl− ion. The Cl− ions are at the cube apices and the Cs+ ions at the cube centers. It can just as well be described by assuming the Cs+ ions are at the apices and the Cl− ions at the centers of the cubes. The NaCl (rocksalt) structure is face-centered cubic, the motif consisting of one Na+ and one Cl− ion (Fig. 8.3b). The Cl− ions are at the apices of the cube and at the face centers, and the Na+ ions at the middle of the sides and one at the center of the cube. The structure can also be described by replacing the Cl− ions by the Na+ ions and vice versa. In the zinc blende (or sphalerite) structure,1 ZnS is face-centered cubic (motif consisting of one Zn2+ ion and one S2− ion), with the S2− ions at the vertices of the cubes and at the face centers (Fig. 8.3c). If the cube is thought to be divided into eight small cubes with half the side, we see that the Zn2+ ions are at the centers of every other of these cubes. As above, the structure can also be described by substituting the S2− ions for the Zn2+ ions and vice versa. We will attempt to “predict” these simple structures with AX formula using the maximum compacity criterion. We saw that the motif is one AX unit. We will therefore consider that the ions of one type (say the negative A ions, and we will see this is reasonable), with radius r− , form a compact lattice of ions (simple cubic ﬁrst, then face-centered cubic), and determine the size of the voids in these structures where the X ions, with radius r+ , could be located. We call a the parameter of the cubic unit cell.

1. It is necessary to specify “blende structure” because ZnS can also crystallize in another form, wurtzite (Exercise 8.3).

170

Symmetry and Physical Properties of Crystals

Primitive cubic lattice The ions located at the cube apices touch each other and their radius r− is equal to a/2. The ion lattice thus formed exhibits voids centered at the centers of the cubes. The radius r+ of the sphere which can be placed at the√center of a cube while touching the ions with radius r− is such that 2r+ = a 3 − a. Hence the ratio of ionic radii should be: r+ √ = 3 − 1 = 0.73. r− The positive ion, at the center of the cube, has eight neighbors at the same distance: it has coordination number 8, and the same applies for the negative ions. Face-centered cubic lattice

√ The ions touch each other along the face diagonals, and r− = a 2/4. There are two kinds of voids: 1.

At the center of the cube: This is called an octahedral site because the ﬁgure formed by the six nearest neighbors located at the face centers is an octahedron, the regular polyhedron with eight faces. We would easily see, by considering the whole lattice, that the same type of site exists at the middle of the sides. Such a face-centered cubic lattice, where2 one type of ions is at the lattice nodes and the other type of ions at the center of the cube and at the middle of the sides, describes the NaCl structure (Fig. 8.3b). The Na+ and Cl− ions have coordination number 6.

2.

At the centers of the eight cubes with side a/2 into which the cube with side a can be divided. These are called tetrahedral sites because the ﬁgure formed by the nearest neighbors is a regular tetrahedron. In such a structure, there are twice as many tetrahedral voids as there are atoms at the apices of the cube and at the face centers, and the AX structure uses only every other void. This is the ZnS structure.

A simple geometrical calculation provides the radius ratios for the two kinds of voids: r+ = 0.41 r− r+ = 0.22 r−

for the octahedral site (coordination number 6), for the tetrahedral site (coordination number 4).

Let us now see how the various voids are ﬁlled depending on the value of the r+ /r− ratio. If r+ /r− = 0.73, the negative ions are at the vertices of the cubes and the positive ions at the centers of the cubes: this is the CsCl structure (Fig. 8.3a). 2. This description implies that we chose to have a lattice node coincide with one type of ion.

Chapter 8 – Chemical bonds and crystal structures

171

The more r+ /r− exceeds the value 0.73, the more the positive ion moves the negative ions apart. If r+ /r− is smaller than 0.73, the positive ion ﬂoats about in the void, and the negative ions rearrange into a face-centered cubic lattice where the positive ion sits in the octahedral void, which it enlarges by moving the negative ions apart (NaCl structure on Fig. 8.3b). If r+ /r− = 0.41, the negative ions touch one another. The more r+ /r− exceeds the value 0.41 (while remaining < 0.73), the more the positive ion pushes the negative ions apart. When r+ /r− is less than 0.41, the positive ion ﬂoats about in the octahedral cavity and the positive ions move to the tetrahedral sites (ZnS-blende structure of Fig. 8.3c), moving apart the negative ions, which come to contact only when r+ /r− further decreases to the value 0.22. To summarize, we obtain the following rule: if r+ /r− > 0.73, CsCl structure; if 0.41 < r+ /r− < 0.73, NaCl structure; if 0.22 < r+ /r− < 0.41, ZnS (blende) structure. This rule is quite well obeyed (Table 8.4). The deviations originate mainly from the fact that the bonds are but rarely purely ionic, in contrast with the starting assumption. There can be for example a covalent contribution, which leads to a tendency for the external electrons not to be distributed with spherical symmetry, so that the starting hypothesis of a spherical ion is no more perfectly satisﬁed. Table 8.4: r + /r − ratios for some crystals with various cubic structures CsCl type

r+ /r−

NaCl type

r+ /r−

CsCl

0.94

KF

1.04

CsBr

0.87

CaO

0.71

CsI

0.77

KBr

0.70

LiF

0.56

ZnS type

r+ /r−

NaCl

0.56

AgI

0.52

CaS

0.54

ZnS

0.40

MgO

0.51

BeS

0.19

LiBr

0.38

8.2.4. Other cubic structures It appears useful to introduce a few other ionic structures, considered as “classic” because many crystals share one or the other of these structures, which are so to speak canonical structures. We chose ﬂuorite CaF2 , rutile TiO2 ,3 and the perovskite structure CaTiO3 . 3. TiO2 also exists in two other forms: anatase (tetragonal) and brookite (orthorhombic).

172

Symmetry and Physical Properties of Crystals

The CaF2 structure is face-centered cubic (Fig. 8.4a). The Ca2+ ions occupy the apices and the face centers of the cube, and the F− ions the eight tetrahedral sites. This structure can also be described as a set of cubes, with sides half the side of the unit cell, where the apices are occupied by a ﬂuorine ion and the center of every other cube by a Ca2+ ion. The ratio of the ionic radii of Ca2+ and F− is equal to 0.74, in good agreement with the coordination number 8 corresponding to a positive ion at the center of a cube whose apices are occupied by a negative ion as for CsCl. However here, since there are twice as many F− ions as Ca2+ ions, the Ca2+ ions are at the centers of every other cube only. The result is a face-centered cubic unit cell.

F

Ca

(a)

Ti

(b)

O

Ca

Ti

O

(c)

Figure 8.4: Three examples of structures representative of many ionic crystal structures: (a) ﬂuorite CaF2 ; (b) rutile TiO2 ; (c) CaTiO3 , the perovskite structure Rutile TiO2 has a tetragonal primitive unit cell (Fig. 8.4b). The Ti atoms are located at the vertices and at the center of the unit cell. Each of the apical Ti atoms is surrounded by two O atoms at the same height, and the Ti atom and its two O neighbors are aligned parallel to one of the diagonals of the square base of the unit cell. The Ti atom at the center of the unit cell also has two O atoms at the same height as itself, but they are aligned parallel to the other diagonal of the square. The perovskite structure, the model of which is CaTiO3 (Fig. 8.4c), is primitive cubic with Ca atoms at the apices of the cube, O atoms at the face centers, and a Ti atom at the center of the cube. The structure of CaTiO3 actually is slightly distorted with respect to this cubic structure. Many substances have this type of pseudo-cubic unit cell, and they often exhibit a high-temperature phase which is exactly cubic. A good example is barium titanate BaTiO3 , which is cubic at high temperature (T > 120◦ C), and undergoes, when temperature decreases, various transitions toward other structures: ﬁrst tetragonal, then orthorhombic and ﬁnally rhombohedral (Exercise 12.7).

Chapter 8 – Chemical bonds and crystal structures

173

8.3. Covalent bonds 8.3.1. Nature of covalent bonds In an elementary presentation, we can say that covalent bonding occurs between two atoms when they share a pair of electrons. In contrast to the ionic bonds, the electron density is no more zero between the atoms. The nature of this bond can only be explained through quantum mechanics. To give a taste of the argument, take the simplest example, that of the H+ 2 ion consisting of two protons and an electron. It can be shown that the wave function of the electron can be written as the combination of the atomic wave functions or “orbitals” Ψ1 and Ψ2 of each of the hydrogen atoms: Ψ± = A± (Ψ1 ± Ψ2 ). The probability density of the electron between the nuclei is non-zero for the Ψ+ combination (called the bonding solution) while that associated to the Ψ− combination (called the antibonding solution) is zero. The energies E + and E − associated to these two states vary as a function of the distance ρ between the protons as shown on Figure 8.5. The energy E + is always smaller than E − , and its minimum value −E0 leads to a cohesive energy equal to E0 . Each state of the bonding orbital can be occupied by two electrons with opposite spins (Pauli’s principle). In the ground state of the neutral hydrogen molecule (H2 ), the electrons of both atoms occupy the bonding state, and they have opposite spins. This is the prototype of the covalent bond, consisting of two electrons with opposite spins, shared between the two bound atoms. If the external electron shell of an atom is several electrons short of being full, this atom can share electrons with several neighboring atoms and thus form several covalent bonds. Each covalent bond then requires the participation of one orbital per bound atom. Energy

E+

E−

0 −E 0

Figure 8.5: Schematic representation of the potential energy of an H+ 2 ion as a function of the distance ρ between the hydrogen nuclei for the bonding orbital, E + , and the anti-bonding orbital, E −

174

Symmetry and Physical Properties of Crystals

8.3.2. Basic property It can be shown that a covalent bond is the more stable the larger the overlap between the wave functions of the two electrons that take part in the bond. The electronic states of isolated atoms do not all have the spherical symmetry of s states. The p states, with 3-fold orbital degeneracy (the total degeneracy, with spin included, is then 6-fold) have wave functions which point along the three axes of an orthogonal referential. There is thus a strong overlap of the p orbitals with the orbitals of the neighboring atoms if the latter are located along these axes. Consider the example of the nitrogen–hydrogen bond in the NH3 molecule. The electronic structure of the nitrogen atom includes two 1s electrons, two 2s electrons and three 2p electrons. The external 2p shell of the nitrogen atom lacks three electrons to be complete. The three p orbitals of the nitrogen atom each form a covalent bond with the spherical 1s orbital of one of the hydrogen atoms. These bonds are almost at right angles to one another. Actually, the angle between two bonds is 107◦ , and the molecule is a pyramid, the base of which is an equilateral triangle and the apical angles are equal to 107◦ . The N atom is at the apex of the pyramid and the H atoms at the apices of the equilateral base. In general, the principle of maximum overlap of wave functions leads to the covalent bonds having preferential directions.

8.3.3. Examples The following examples are monoatomic crystals. The bonds therefore connect atoms of the same type. Diamond It consists of carbon atoms. The electronic structure of the outermost shell of carbon (n = 2) consists of two 2s electrons and two 2p electrons. It lacks four electrons to be full. The four electrons of the n = 2 shell form hybrid orbitals consisting of linear combinations of the s, px , py and pz orbitals. These orbitals, called sp3 , are oriented along the directions that connect the center of a regular tetrahedron to its four apices. In a diamond crystal, each carbon atom is thus connected to four neighbors by tetrahedral bonds (Fig. 8.6). The diamond crystal can be considered as a giant molecule, with practically inﬁnite extent. Silicon and germanium crystals have the same structure as diamond. Their outermost shell (n = 3 for Si and n = 4 for Ge) also includes 4 electrons (two s electrons and two p electrons). Generally, consider atoms in which the outermost shell would have 8 electrons if it were saturated. If this shell actually contains N electrons, the external shell will be saturated if 8 − N covalent bonds are formed. Each bond then uses one of the N electrons of the neighboring atom (an atom of the same type

Chapter 8 – Chemical bonds and crystal structures

175

in the monoatomic crystals to which we restrict discussion), and this requires N ≥ 8 − N , hence N ≥ 4. The following paragraphs successively discuss a case where N = 5, then a case with N = 6. An example with N = 7 is treated in Section 8.4.2.

Figure 8.6: Crystal structure of diamond Arsenic The outermost electronic shell (n = 4) contains two 4s electrons and three 4p electrons, hence a total of ﬁve electrons. Three pseudo-plane bonds are then formed, and the pseudo-planes can be described as corrugated planes. An atom located in the zero height plane is connected to three atoms at height 1.37 Å as shown on Figure 8.7, which represents the projection of these atoms onto the plane at height zero. The arrows indicate the direction of increasing height on the bonds. The angle between bonds is 94.1◦ (instead of 120◦ as expected for coplanar bonds). The next corrugated plane is at height 3.516 Å and its projection is displaced with respect to the ﬁgure by vector AB. The “corrugated” planes are bound to one another by Van der Waals bonds (see next section).

A

B

3.76 A°

Figure 8.7: Arsenic crystal; structure of a pseudo-plane of atoms. The atoms represented by empty circles are at height zero and those represented by full circles at height 1.37 Å. Selenium The outermost electronic shell (n = 4) contains six electrons (two 4s electrons and four 4p electrons), and each Se atom must therefore share two bonds. They are at an angle of 103.1◦ to each other. The “inﬁnite molecule” is a chain (Fig. 8.8). The positions of the atoms in one chain are deduced from

176

Symmetry and Physical Properties of Crystals

one another by the symmetry elements of a 31 screw axis. These helix-shaped chains are stacked parallel to one another and they are bound to one another by Van der Waals forces. 1⁄3

1⁄3 0

0

2⁄3

C

2⁄3

b 1⁄3

1⁄3 0

a

2⁄3

(a)

0 2⁄3

(b)

Figure 8.8: Selenium crystal: (a) structure of a chain of atoms and its 31 screw axis; (b) hexagonal unit cell projected on its basal plane, with the height of the atoms expressed in units of the lattice parameter c

8.3.4. Conclusion 1.

Covalent bonds are oriented: this is their main characteristic.

2.

The distance between two given atoms engaged in a covalent bond is well deﬁned. For example, the C–C distance in a diamond crystal is equal to that between carbons in the single bond of ethane (C2 H6 ), 1.54 Å.

3.

The order of magnitude of the energy of these bonds is a few eV. Examples are given in Table 8.5. Table 8.5: Energy of some covalent bonds. The C–C bond considered is a single bond.

Energy (in eV) 4.

H–H

C–C

Si–Si

Ge–Ge

4.5

3.6

2.3

1.9

There are many solids where the bonds are not totally covalent but partly ionic: they are referred to as iono-covalent bonds. The atoms engaged in these bonds always ﬁll their outermost electronic shell.

Chapter 8 – Chemical bonds and crystal structures

177

8.4. Van der Waals bonds, or molecular bonds 8.4.1. Nature and properties The simplest example is that of the rare gases, consisting of neutral atoms with their outermost electronic shell full. Although the atoms are neutral, the Van der Waals force is electrostatic in origin. These atoms do not have a permanent electric dipole moment (P(t) = 0) but the dipole moment oscillates around its average zero value. At a given time P(t) is therefore non-zero, and it creates an electric ﬁeld at the position of the neighboring atom, which it polarizes. The interaction energy between the two atoms can be calculated. It is found to be negative, with absolute value proportional to 1/r 6 , whence an attractive force varying as 1/r 7 . The order of magnitude of the Van der Waals type bond energies is 0.1 eV. There is no restriction on the angles between bonds, which may have any orientation. Van der Waals radii: They can be determined from the contacts between identical atoms bound by Van der Waals forces. Then, knowing a number of these radii, we can determine the others by examining the distances between atoms of diﬀerent types bound by a Van der Waals force.

8.4.2. Example Van der Waals bonds appear in all crystals where the elementary building block is a molecule. A very simple example is the chlorine crystal (Fig. 8.9). 0

½

0

c

0

½

0

½

0

½

b 0

½

0

½

0

½

0

½

0

Figure 8.9: Orthorhombic crystal of chlorine: projection of the atoms onto a plane perpendicular to basis vector a. The lines connecting two chlorine atoms represent the covalent bonds.

178

Symmetry and Physical Properties of Crystals

The outermost shell of the chlorine atom has 7 electrons, and the atom can covalently bond only to one neighbor to form a Cl2 molecule. The crystal consists of Cl2 molecules connected by Van der Waals forces. This is called a “molecular crystal”. The molecule is extremely simple in this case, but in general the molecules can contain a great number of atoms and have complicated, irregular shapes. Their most compact stacking is not easily determined, all the more since other factors can play a part, for example local charges which create a local electric ﬁeld in their vicinity.

8.5. Metallic bonds 8.5.1. Nature and properties In a pure metal, the atoms are all identical and the bond cannot be ionic. Also, the number of electrons in the outermost shell of a metal atom is smaller than 4, and the bond cannot be covalent. The nature of the metallic bond can be understood starting from the crystal structure (as evidenced by X-ray diﬀraction), and describing quantum mechanically the behavior of an electron in the periodic potential of the metal ions that form the crystal lattice. It can then be shown, for the electrons in a crystal, that there is a set of energy levels forming a continuous band called the conduction band. The electrons in the conduction band behave almost like free electrons, and they also provide the bonding between all the atoms. The crystal structures observed are well explained by a model of hard spheres with compact (close-packed) stacking. The radius of the spheres is calculated as half the distance between neighboring atoms, as deduced from the crystal structure determined by X-ray diﬀraction. The radius of the metallic ions thus determined is always larger than the radius of the corresponding ion in an ionic crystal. For example the radius of the Na+ ion is equal to 1 Å while the radius of Na metal is 1.86 Å. The interpretation is that, in NaCl for example, the Na+ ions are attracted by the Cl− ions and therefore get as close as they can to them. In metallic Na, the Na+ ions are repelled, cohesion being due to the conduction electrons. The cohesive energy of a metal is of the order of 1 eV per atom (except for the transition metals).

8.5.2. Examples The maximal compacity of a stacking of identical hard spheres is obtained for the face-centered cubic and close-packed hexagonal structures.

Chapter 8 – Chemical bonds and crystal structures

179

Consider two spheres with radius a, touching each other. A third sphere contacting these two spheres will form with the two ﬁrst ones an equilateral triangle. A plane of contacting spheres, where the centers are designated as A, form a lattice of plane hexagonal unit cells (Fig. 8.10a), and the lines connecting the centers of the spheres form a set of equilateral triangles. A sphere will position above this plane in the most compact way possible if its center projects at the center of any one of these equilateral triangles. Since there are twice as many centers of equilateral triangles as there are spheres in the compact starting plane, the contacting spheres in the second plane will project on every other of these two sites, which we call B. We will call C sites those which project on the other centers of equilateral triangles. The spheres of the third compact plane can now project either on the C sites or on the A sites. In the ﬁrst case the crystal will consist of the succession of planes ABCABCABC. . . , while in the second case the succession will be ABABABAB. . . It is easy to show (Exercise 8.1) that the atoms corresponding to succession ABCABC. . . form a face-centered cubic lattice (the motif consisting of a single atom). The planes A, B and C are parallel to the (111) planes of this structure. In the case of the ABABAB. . . sequence, the atoms form a hexagonal lattice. The a and b vectors of the hexagonal lattice are the basis vectors of the plane hexagonal starting lattice. Vector c, perpendicular to a and b, has for its length the distance between two successive A (or B) planes. A simple geometrical calculation (Exercise 8.2) shows that the c/a ratio is then 2 2/3 = 1.63.

b

b a

(a)

A B C

a

(b)

Figure 8.10: Compact stacking of spheres: (a) plane of contacting spheres; (b) projection onto this plane of the atom positions in the neighboring planes Table 8.6 shows that most metal structures are indeed either face-centered cubic or hexagonal, but in the latter case with more or less compacity. However there are also body-centered cubic (I) structures. Some metals are polymorphic, i.e. they feature various structures depending on temperature: this is the case for iron, where γ Fe has an F lattice and α Fe an I lattice. It turns out, when calculated, that the ionic radii are in this case close to each other.

180

Symmetry and Physical Properties of Crystals Table 8.6: Structure and lattice parameters of some metals Face-centered cubic lattice

Body-centered cubic lattice

Hexagonal lattice

Element

a (Å)

Element

a (Å)

Element a (Å)

c (Å)

c/a

Ag

4.086

Cr

2.884

Be

2.287

3.583

1.566

Al

4.050

Fe α

2.8665

Co α

2.507

4.069

1.623

Au

4.078

Li

3.509

Cr

2.722

4.427

1.626

Co

3.548

Mo

3.147

Mg

3.209

5.210

1.624

Cu

3.615

Na

4.291

Ni

2.65

4.33

1.634

Feγ

3.591

Nb

3.300

Ti

2.95

4.686

1.588

Ni

3.524

Zr

3.62

Zn

2.665

4.947

1.856

8.6. Remarks and conclusions We described the various types of bonds between atoms in a crystal. However, bonds are not always of a perfectly well-deﬁned type. In particular, covalent and ionic bonds are only the extreme terms of a set of bonds featuring both an ionic and a covalent character. Also, several types of bonds can appear together in a crystal: we saw examples of coexistence of covalent binding and Van der Waals binding in crystals of arsenic, selenium and chlorine. To conclude, we give two examples of simple crystals exhibiting strong anisotropy because they consist of plane layers bound to one another by weak Van der Waals bonds while the binding within the layers have mixed character and higher energy by at least an order of magnitude. Graphite crystal It consists of carbon atoms each of which is connected to three other carbon atoms by covalent bonds (sp2 hybridization between the s, px and py orbitals), within planes with hexagonal structure (Fig. 8.11). The fourth valence electrons, with orbital pz , of two neighboring atoms bind to each other through a mainly covalent bond. This bond is partly metallic and is delocalized along the plane. This partly metallic character explains the non-negligible electrical conductivity measured along these planes (see Sect. 9.3.1). The inter-plane binding is Van der Waals type.

Chapter 8 – Chemical bonds and crystal structures

181

3.35 Å

1.42 Å

Figure 8.11: Structure of graphite GeS2 crystal The layers consist of a set of tetrahedra. The center of each tetrahedron is occupied by a germanium atom, and the apices by sulfur atoms. Within a layer, the Ge atoms form a plane, and the tetrahedra are connected to one another through their apices. Each sulfur atom at the apex of a tetrahedron is thus connected to two Ge atoms. The Ge–S bonds are iono-covalent, and the layers are bound to one another by Van der Waals forces.

8.7. Exercises Exercise 8.1 Lattice for an ABCABC close-packed stacking. Comparison of Figures 8.10b and 3.14c shows that the spheres in an ABCABC stacking form a rhombohedral lattice. Show that this rhombohedral lattice is a face-centered cubic lattice. Exercise 8.2 Lattice for an ABABAB close-packed stacking 1.

In this stacking the centers of a sphere in plane B and of its three contacting spheres in plane A form a regular tetrahedron with side a equal to the length of the basis vector a of the hexagonal unit cell. Determine, as a function of a, the distance h between planes A and B.

2.

Calculate the c/a ratio for the hexagonal unit cell of the ABABAB lattice.

Exercise 8.3 Tetrahedral sites In the close-packed stacking modes ABCABC and ABABAB, one atom in a given layer and its three nearest neighbors in the adjacent layer form a regular tetrahedron.

182

Symmetry and Physical Properties of Crystals

1.

Calculate the distance d between the center of this tetrahedron and each of its apices.

2.

A spherical atom (or ion), with radius r1 , is placed at the center of this tetrahedron so that it contacts the atoms of the close-packed stacking with radius r2 . Calculate the ratio r1 /r2 .

3.

Wurtzite is a crystal form of ZnS diﬀerent from blende. Its lattice is hexagonal, with a = 3.811 Å, c = 6.234 Å. The atom positions in the unit cell are: Zn

0, 0, 0

S

0, 0, u

1 3, 1 3,

2 3, 2 3,

1 2 1 2

+u

and

u ≈ 0.375.

Show that the sulfur atoms are practically in the tetrahedral sites of a structure in which the centers of the Zn atoms form an ABABAB stacking. Compare this to the blende structure described in Section 8.2.3.

Chapter 8 – Chemical bonds and crystal structures

183

Complement 8C. Magnetic structures Understanding the physics of magnetic materials requires a knowledge not only of their crystal structure but also of their magnetic structure. The crystal structure indicates the shape and dimensions of the unit cell, the positions of the various individual ions or atoms, and the extent of their thermal vibration. The magnetic structure describes the size and orientation of the magnetic moment carried by some of the ions. Materials are often designated as magnetic when they react strongly to an applied ﬁeld. This usually means that they contain permanent magnetic moments which are, below a transition temperature, ordered. The simplest magnetic materials are ferromagnets: below TC , the Curie temperature, all the magnetic moments are, within a magnetic domain,4 parallel (Fig. 8C.1a).

(a)

(b)

(c)

(d)

Figure 8C.1: Schematic representation of the magnetic moment arrangements, on a microscopic scale, in ferromagnets (a), ferrimagnets (b) and antiferromagnets (c). In these ﬁgures, each arrow represents an atomic magnetic moment. Figure (d) shows, on a macroscopic scale, an arrangement of magnetic domains in a ferromagnet: each arrow then represents the direction of the spontaneous magnetization:5 the scale of this ﬁgure could be anywhere between micrometers and millimeters.

4. A magnetic domain is a macroscopic region of the sample where the orientation of the spontaneous magnetization, hence of the magnetic moments, is uniform. There are always at least two opposite (time-reversed) directions for the magnetic moments, as in uniaxial materials. The number of equivalent domains is set by the ratio of the magnetic point symmetry of the material above and below the Curie temperature, and it depends on what crystallographic direction the moments spontaneously take. For example, when the material is cubic above the Curie temperature and the spontaneous magnetization directions are <100>, as in slightly silicon-alloyed iron, there are 6 families of magnetic domains (spontaneous magnetization along ±[100], ±[010], ±[001]) (Fig. 8C.1d). The magnetization process, under the inﬂuence of an applied magnetic ﬁeld, starts with the growth of the favorably oriented domains. 5. The magnetization is the magnetic moment per unit volume. It is analogous to the polarization in dielectrics, discussed in Chapters 9 and 15.

184

Symmetry and Physical Properties of Crystals

Examples of ferromagnets are iron, cobalt, nickel and many of their alloys or compounds. Another important class of magnetic material comprises the ferrimagnets (Fig. 8C.1b), in which the magnetic moments of one type of ions are “up”, and those of another type of ions, with a diﬀerent value of the moment, are “down”, yielding a resulting non-zero (spontaneous) magnetization at the scale of a domain. Examples are the ferrites used in high-frequency transformer cores, or as permanent magnets. The order feature is shared by some materials which do not react strongly to a magnetic ﬁeld and are therefore not obviously attractive for applications. These have, below the ordering temperature (the Néel temperature TN ), as many “up” as “down” magnetic moments with the same modulus, and therefore zero overall spontaneous magnetization. These materials, the simpler examples of which are NiO, CoO and MnO, or MnF2 , CoF2 and NiF2 , are called antiferromagnets (Fig. 8C.1c). The prime tool for investigating the magnetic structure of materials is neutron diﬀraction. Neutrons (see Complement 4C) interact with the nuclei (the nuclear interaction) and, since they carry a magnetic moment, they also sense magnetic ﬁelds. In the wavelength range used for diﬀraction by the microscopic structure of materials, on the order of 10−10 m, they are diﬀracted by the microscopic-scale variation of the magnetic ﬁelds in matter, and the probability of magnetic scattering happens to be of the same order of magnitude as for nuclear scattering. From this information, the distribution of magnetic moments that gives rise to these ﬁelds can be determined. For example, in some simple antiferromagnets (CoO, NiO or MnO), the magnetic period, in the direction along which the moments alternate, is double that of the chemical structure, because chemically identical ions have alternately up and down orientations. The neutron diﬀraction pattern will therefore feature new, purely “magnetic” reciprocal lattice nodes and diﬀraction peaks, which vanish above the Néel temperature. Just as the symmetry of the crystal structure is described by one of the 230 space groups, the magnetic symmetry is described by one of the 1651 magnetic groups. The 32 crystallographic point groups are replaced by 122 magnetic point groups. The central addition to the toolbox of structure symmetry elements is the operation called “time reversal”. The notion under this provocative term is actually simple. Microscopic magnetic moments are represented by axial vectors (see Sect. 10.6). They are due to the equivalent of current loops, i.e. of circulating electric charge. Reversing the magnetic moment is tantamount to reversing the velocity of the charges, as if a movie were being played backwards, or if time were ﬂowing backwards. Thus the magnetic symmetry involves operations such as m (mirror combined with reversal of the magnetic moment, which can be described as time reversal), and the magnetic Bravais lattice description can feature notations such as Ip , meaning anti-centering, i.e. the combination of displacement by half the unit cell diagonal and magnetic moment reversal.

Chapter 8 – Chemical bonds and crystal structures

185

Actually, X-rays also interact, albeit weakly, with the magnetic moments. With synchrotron radiation X-rays, valuable complementary information can be extracted on magnetic structures: magnetic X-ray scattering can reveal the two contributions (spin and orbital) to the magnetic moment, whereas magnetic neutron diﬀraction is sensitive only, via the magnetic ﬁeld it creates, to the total magnetic moment.

Further reading D.H. Ryan, Neutron Powder Diﬀraction Studies of Magnetic Materials. Powerpoint document, prepared for the 2009 summer course of the Canadian Institute for Nuclear Scattering; available on the web at www.cins.ca/docs/SS09 (click on DHR CNBC June09.ppt) M. de Graef, Teaching crystallographic and magnetic point group symmetry using three-dimensional rendered visualizations, International Union of Crystallography, Teaching Pamphlets; http://www.iucr.org/ data/assets/pdf ﬁle/0006/13929/ﬁnal 23.pdf J. Rodríguez-Carvajal and F. Bourée, Symmetry and magnetic structures, in Contribution of Symmetries in Condensed Matter, ed. by B. Grenier, V. Simonet and H. Schober. Proceedings of spring school held at Presqu’île de Giens, France, in May 2009. EDP Web of Conferences, vol. 22 (2012). Available on the web, at http://dx.doi.org/10.1051/epjconf/20122200010

186

Symmetry and Physical Properties of Crystals

References [1] G. Schoknecht, Z. Naturforsch. 12A, 983 (1957) [2] V.M. Goldschmidt, T. Barth, G. Lunde, W.H. Zachariasen, Skr. Norske Vidensk. Akad. Skrifter I Mat. Naturv. Kl. 2, 1 (1926) [3] L. Pauling, J. Am. Chem. Soc. 49, 765 (1927) [4] R.D. Shannon, C.T. Prewitt, Acta Cryst. B25, 925 (1969) [5] W.G. Wyckoﬀ, Crystal Structures, vol. 1 (Wiley, 1963)

Chapter 9

Crystal anisotropy and tensors This chapter shows why the anisotropy of crystals requires a representation of their physical properties by tensors, and deﬁnes them. It then shows how the symmetry of a given crystal (its point group) inﬂuences the form of these material tensors. Curie’s and Neumann’s principles and their application to the tensor properties of crystals are presented in Section 9.5.

9.1. Introduction The physical properties of crystals belong to either of two broad categories: intrinsic and extrinsic properties. The intrinsic physical properties are identical in various samples of a given material because they depend on the very nature of the material: its chemical composition, the nature of the bonds between atoms and their structural arrangement. Examples of intrinsic properties are: thermal expansion and elastic properties, which reveal on a macroscopic scale the forces between neighboring atoms, the type of electrical conductivity (insulating or conducting or semiconductor), which is related to the nature of the chemical bonds between atoms. A good example is carbon, an insulator when it crystallizes in the form of diamond, while its other (polymorphic) form, graphite, is a conductor. The extrinsic properties are related to the existence of defects in the crystal, and they can therefore vary extensively between samples. Two examples are: plastic deformation: here, in contrast to elastic deformation, the sample does not return to its initial state when the force which created the strain is removed. Plastic deformation is related to the existence and multiplication of linear defects, called dislocation lines (or, for short: dislocations), whose initial number and nature vary from sample to sample depending on the growth process and on the previous deformation. A brief introduction to dislocations is given in Complement 13C.

© Springer Science+Business Media Dordrecht 2014 C. Malgrange et al., Symmetry and Physical Properties of Crystals, DOI 10.1007/978-94-017-8993-6_9

187

188

Symmetry and Physical Properties of Crystals the value of the electrical conductivity of a semiconductor, which depends on the density of impurities (which means, when it is deliberate, the extent of doping) in the sample.

In this book, we only consider intrinsic physical properties of crystals. In the ﬁrst part, we saw that crystals are formed from the periodic repetition of the crystal motif, at the microscopic scale, along three non-coplanar directions. A direct consequence of this periodicity is the anisotropy of the physical properties of crystals, which depend on the direction in which a constraint is applied and on the direction in which the resulting eﬀect is measured. The description of this anisotropy involves special mathematical objects, called tensors. This is why this second part of the book starts with two general chapters which analyze the notion of tensor, describe the general properties of tensors, and show how the symmetry of an individual crystal makes it possible to reduce the number of independent coeﬃcients of any tensor representing one of its intrinsic physical properties. The following chapters describe speciﬁc physical properties, mainly mechanical and optical.

9.2. Anisotropic continuous medium The physical properties discussed in this second part of the book are macroscopic properties. In describing them, the crystal is considered as a continuous and anisotropic medium. To satisfy the assumption of continuity, we must assume that any elementary volume V fulﬁlls two conditions. It must contain enough unit cells that it may be considered as homogeneous, but it also must be small enough that the variations of an external applied ﬁeld within this volume be negligible. When these external ﬁelds are sine waves (electric ﬁeld E or magnetic ﬁeld B. . . ), the characteristic length is their wavelength λ. The elementary volume V must therefore have dimensions very much smaller than this wavelength. The two above conditions can be summarized by the double inequality: √ 3 a V λ where a is the largest one among the parameters of the crystal unit cell. This means that, if the wavelength of the applied ﬁelds is much larger than the dimensions of the unit cell, the variations of the ﬁeld within the elementary volume can be neglected, and the crystal can be viewed as a continuous medium. Furthermore, the cell parameters can be considered as inﬁnitely small with respect to the relevant volume, and the same applies even more to fractions of these parameters. It is therefore no more justiﬁed to distinguish between pure and screw rotation axes, or between pure and glide mirrors, since the translations associated to these symmetry elements are fractions of a lattice parameter (see Sect. 7.2.1 and 7.2.2). In other words, the eﬀect of the crystal’s symmetry on its macroscopic properties will be described by its point group and not by its space group.

Chapter 9 – Crystal anisotropy and tensors

189

Conversely, if the wavelength of the ﬁeld applied to the crystal is on the same order of magnitude as its lattice parameter (X-ray range), the crystal can no more be considered as continuous. Its discrete structure must be taken into account, and indeed such probes can be used to investigate the crystal structure and thus the space group of the crystal. Our discussion of the physical properties will involve either static constraints (mechanical properties), or periodic constraints with wavelengths larger by several orders of magnitude than the lattice parameters (acoustic waves and optical electromagnetic waves). The crystal can thus be considered as an anisotropic continuous medium, and crystal symmetry aﬀects the physical properties through the point group of the crystal.

9.3. Representing a physical quantity by a tensor Some physical quantities are independent of any notion of orientation: this is the case for temperature or the mass per unit volume of a material. They are expressed by a scalar. Others are expressed by a vector, for example an electric ﬁeld or the polarization of a crystal under the inﬂuence of this ﬁeld. Consider two vector-type physical quantities, A and B, related by a linear law. In a gas or liquid, this relation is written as A = γB where γ is a scalar. A and B are then parallel. In a crystal, A is generally not parallel to B, and a tensor must be introduced to describe the physical quantity γ. This will be analyzed in detail on the basis of an example in the next section (Sect. 9.3.1). Tensors, in the same way as vectors which, as we will see, are just a special form of tensors, are deﬁned by their components in a given system of axes. It is simpler, and this will be done throughout this book, to select for this use not the set of crystal axes (basis {a, b, c}), but an orthonormal set of axes (Ox1 x2 x3 ) (basis {e1 , e2 , e3 }), usually chosen as close as possible to the crystal axes. For example, in the case of the crystal systems with an orthogonal unit cell (orthorhombic, tetragonal, cubic), the orthonormal set of axes (Ox1 x2 x3 ) in which we express the tensor is chosen parallel to the vectors a, b, c that deﬁne the unit cell. For crystals with a hexagonal unit cell, one of the axes is chosen parallel to the 6-fold axis of the lattice, etc.

9.3.1. Example: electrical conductivity Electrical conductivity is a good example for understanding the eﬀect of crystal anisotropy on the physical properties of a crystal. An electric ﬁeld E applied to a conductor induces a current density j within the material. The motion of free charges is then characterized by the electrical conductivity σ through j = σE where σ is a scalar if the material is isotropic.

(9.1)

190

Symmetry and Physical Properties of Crystals

To illustrate this relation, imagine we are performing conductivity measurements on two very diﬀerent samples of graphite: a compacted graphite powder, and a single crystal of graphite. The crystal structure of graphite, as described in Chapter 8 (Fig. 8.11), consists of a stacking of equidistant dense planes, with hexagonal symmetry, called graphitic planes, connected by Van der Waals bonds. In the ﬁrst experiment, performed on compacted powder, we apply an electric ﬁeld E in any direction. The current density turns out to be parallel to E whatever the direction of the applied ﬁeld E, and proportional to the norm of E. The conductivity σ is then a scalar. In this case, the powder behaves with respect to the applied electric ﬁeld like an isotropic material. The powder consists of many small crystals, randomly oriented relative to one another, and thus the inﬂuence of structural anisotropy on the measured physical property disappears. Now consider the single crystal of graphite. Due to the special structure of this material, very diﬀerent values of the current density will be obtained depending on the orientation of the applied electric ﬁeld. A strong current density will be measured if the ﬁeld is applied along a direction in the graphitic planes, and a weak current density will be obtained with the ﬁeld perpendicular to the graphitic planes (Sect. 8.6). The ratio between these values varies between 102 and 105 depending on crystal quality [1]. If the applied ﬁeld has a general direction, the current density has no reason to be parallel to the ﬁeld, and the three components of j can be expressed as a function of those of E through the linear relations: j1 = σ11 E1 + σ12 E2 + σ13 E3 j2 = σ21 E1 + σ22 E2 + σ23 E3

(9.2)

j3 = σ31 E1 + σ32 E2 + σ33 E3 , where ji and Ei with i = 1, 2, 3 are the components of j and E respectively, in an orthonormal set of axes (Ox1 x2 x3 ). These three relations can also be written ji =

3

σik Ek

k=1

or, using Einstein’s condensed notation, also referred to as Einstein’s convention: ji = σik Ek . This convention consists in suppressing the sum sign, which becomes implicit, before a product of factors when the sum is performed over a subscript that appears twice in the product. Here the summation is performed over subscript k (called the dummy subscript, or dummy index), which appears in σik and in Ek . The subscript i, which is not summed over, is called the free subscript, and it must appear on both sides of the equal sign. We will always use this notation in what follows.

Chapter 9 – Crystal anisotropy and tensors

191

Equations (9.2) can also be written in the following matrix form: ⎞ ⎛ ⎞⎛ ⎞ ⎛ σ11 σ12 σ 13 E1 j1 ⎝ j2 ⎠ = ⎝ σ21 σ22 σ23 ⎠ ⎝ E2 ⎠ . j3 σ31 σ32 σ33 E3 Electrical conductivity clearly appears as a table of 3 × 3 = 9 components of a quantity described as a tensor quantity. The nine numbers that deﬁne it depend on the axis system chosen to express the components of vectors E and j. It is therefore essential to understand how this table transforms when the vectors E and j are expressed in another orthonormal coordinate system. In other words, we must determine the relation that makes it possible to go over from table σik , obtained when the vectors E and j are expressed in a obtained when the same vectors are given orthonormal frame, to the table σik expressed in another orthonormal frame.

9.3.2. A refresher on orthonormal frame changes Let R be a frame deﬁned by the orthonormal basis {e1 , e2 , e3 } and R a new frame deﬁned by the orthonormal basis {e1 , e2 , e3 }. The new basis vectors can be expressed as a function of the old ones through the relations: ei = aij ej

(9.3)

where we use Einstein’s convention as deﬁned in the section above: summation over the subscript j which appears twice is implicit. We immediately see that: aij = ei · ej .

(9.4)

Equation (9.3) can be represented through the table below: e1

e2

e3

e1

a11

a12

a13

e2

a21

a22

a23

e3

a31

a32

a33

In this table akl = ek · el . We note that aji = ej · ei is the projection of ei onto ej , so that: ei = aji ej .

(9.5)

192

Symmetry and Physical Properties of Crystals

A vector x can be expressed in basis {e1 , e2 , e3 } through relation: x = x1 e1 + x2 e2 + x3 e3

or

x = xi ei

(9.6)

or

x = xj ej .

(9.7)

and in basis {e1 , e2 , e3 } through x = x1 e1 + x2 e2 + x3 e3

Taking relation (9.5) into (9.6), we obtain x = xi aji ej and, comparing with (9.7), we obtain xj = aji xi .

(9.8)

In the same way, taking (9.3) into (9.7) and comparing with (9.6), we obtain xj = aij xi .

(9.9)

Transformation from one orthonormal frame to another orthonormal frame leads to the two following relations, (9.10) and (9.11): aih aik = δhk

(9.10)

where δhk is Kronecker’s symbol, equal to 1 if h = k and to 0 if h = k. The proof is that eh · ek = δhk = aih ei ajk ej = aih ajk δij = aih aik . In the same way, using the fact that eh · ek = δhk , we obtain ahi aki = δhk .

(9.11)

Let us designate as A the matrix {aij }, where i is the subscript for the row and j for the column. The i-th row of this matrix consists of the components of the new basis vector ei in terms of the old basis vectors. This matrix A is called the transformation matrix for going over from the orthonormal coordinate system R, with basis {e1 , e2 , e3 }, to the orthonormal system R with basis {e1 , e2 , e3 }. Two simple examples of transformation matrices are given below: 1.

The new frame R is the symmetric of R with respect to a plane perpendicular to axis Ox2 (Fig. 9.1a). In this case, the vectors e1 , e2 , e3 are given by e1 = e1 ,

e2 = −e2 ,

and the transformation matrix for ⎛ 1 A=⎝ 0 0

e3 = e3

this change of frame is given by ⎞ 0 0 −1 0 ⎠ . 0 1

Chapter 9 – Crystal anisotropy and tensors 2.

193

The new frame R is deduced from frame R through a rotation by angle ϕ around axis Ox2 (Fig. 9.1b). In this case, the vectors e1 , e2 , e3 are given by: e1 = cos ϕ e1 − sin ϕ e3 ,

e2 = e2 ,

and the transformation matrix for ⎛ cos ϕ A=⎝ 0 sin ϕ

e3 = sin ϕ e1 + cos ϕ e3

this change of frame is given by: ⎞ 0 − sin ϕ ⎠. 1 0 0 cos ϕ

x2

O M

x’3 x3

x 2 x’2

x’1 x1

O

x1

x3

x’1

x’3

x’2

(a)

(b)

Figure 9.1: Change in coordinate system. The new frame R (Ox 1 x 2 x 3 ), drawn in dotted lines, is obtained from the initial frame R (Ox 1 x 2 x 3 ), drawn in solid lines, through: (a) symmetry with respect to a plane M perpendicular to axis Ox 2 , (b) rotation by angle ϕ around axis Ox 2 .

9.3.3. Application to electrical conductivity In frame R {e1 , e2 , e3 }, the components jk of j can be written as a function of the components El of E: jk = σkl El . We want to express the coordinates ji of j in frame R as a function of the coordinates Ej of E in this frame. Using relations (9.8) and (9.9), we obtain: ji = aik jk = aik σkl El = aik σkl ajl Ej . E . Therefore The relation we want is ji = σij j = aik ajl σkl . σij

(9.12)

We note here for the last time that Einstein’s convention implies summing over the subscripts k and l which appear twice in the product.

194

Symmetry and Physical Properties of Crystals

Let x and y be two vectors with coordinates respectively xi and yi in basis {e1 ,e2 ,e3 }. Their coordinates xi and yi in basis {e1 , e2 , e3 } are given by xi = aik xk , yj = ajl yl . The product of two coordinates xi and yj takes the form xi yj = aik ajl xk yl , and a relation similar to that of Equation (9.12), connecting components σij σij . Thus, a coeﬃcient σij transforms in a change of axes like the product of two vector components.

9.4. Tensors 9.4.1. Deﬁnition of a tensor The last remark above allows us to understand the following deﬁnition of tensors: A tensor of rank n is (when three-dimensional space is considered) a set of 3n components, characterized by n subscripts, which transform in the change from one orthonormal frame to another orthonormal frame like the product of n vector components. For example, a tensor [T ] of rank 2 (also designated as a second-rank tensor), is a set of 9 coeﬃcients Tij deﬁned in an orthonormal frame R, and called the components of the tensor. In another orthonormal frame R , deduced from R through the transformation matrix {aij }, they become the components Tij such that Tij = aik ajl Tkl

(9.13a)

. Tij = aki alj Tkl

(9.13b)

and conversely:

The tensor as an entity is denoted by a letter, set between square brackets, e.g. [T ]. In the same way, a third-rank tensor [T ] has 27 components Tijk which transform in the same frame change according to relation = ail ajm akn Tlmn Tijk

(9.14a)

. Tijk = ali amj ank Tlmn

(9.14b)

and conversely:

Chapter 9 – Crystal anisotropy and tensors

195

Again in the same way, a fourth-rank tensor [T ] transforms in a change of frame according to = aim ajn akp alq Tmnpq Tijkl

(9.15a)

. Tijkl = ami anj apk aql Tmnpq

(9.15b)

and conversely:

We deduce immediately that a scalar is a tensor of rank 0 and that a vector is a tensor of rank 1. In practice, ascertaining the tensor character of a quantity deﬁned by 3n components implies checking that, in a change of frame, the components transform like the product of n components of vectors. The above deﬁnition restricts the general deﬁnition of tensors (see e.g. the books by Sands [2] or by Schwartz [3]) to the case of orthonormal frames.1 It makes the presentation of tensor physical properties of crystals much simpler while retaining the physics of the phenomena. In practice, problems of crystal physics are almost invariably treated with orthonormal frames.

9.4.2. An important property The derivation used to ﬁnd how the components of the electrical conductivity transform in a change of frame depends only on the vector nature of the quantities E and j and not on their physical nature. We can thus conclude that: If two vector physical quantities A and B, with components Ai and Bj in a given orthonormal axis system, are related by Bi = Tij Aj , then the physical quantity represented by the 9 coeﬃcients Tij is a tensor. With such a relation, we can state that Tij is a second-rank tensor [T ], and we can write B = [T ]A. We use the notation between square brackets to emphasize the tensor nature of the coeﬃcients Tij . More generally, it can be shown that A physical quantity relating a tensor physical quantity of rank p (which will be called the cause) to another tensor physical quantity of rank q (called the eﬀect) is represented by a tensor of rank n = p + q. Let us demonstrate this using an example. Suppose relation Ti = Uikl Vkl connects, in an orthonormal axis system (Ox1 x2 x3 ), tensor cause [V ], with rank 2, to tensor eﬀect T (a rank-one tensor, hence actually a vector) through the coeﬃcients Uikl . In another orthonormal axis system (Ox1 x2 x3 ), deduced from the former through the transformation 1. Using non-orthonormal axes requires the use of covariant and contravariant components, which we do not ﬁnd necessary here.

196

Symmetry and Physical Properties of Crystals

matrix {aij }, the components of T and [V ] are Ti and Vkl , related to the former ones through: = ami Ti , Tm

Vkl = ank apl Vnp

whence we deduce: = ami Ti = ami Uikl Vkl = ami Uikl ank apl Vnp Tm

so that = ami ank apl Uikl Vnp Tm = Umnp Vnp with Umnp = ami ank apl Uikl . This relation shows that Uikl is a tensor of rank 3 = 2+1.

The method we used applies whatever the ranks p and q of the cause and eﬀect tensors are. In what follows, we will frequently use this property to assert that a set of coeﬃcients indeed represents a tensor. We note that the relative electrical permittivity [ε] of a material is a secondrank tensor since it relates the induction D in the material to the electric ﬁeld E, i.e. D = ε0 [ε]E or Di = ε0 εij Ej where ε0 is the permittivity of vacuum.

9.4.3. Field tensors and material tensors Let us return to the example of electrical conductivity ji = σij Ej . This relation connects a cause, here the electric ﬁeld E, to an eﬀect, the current density j, through the electrical conductivity tensor [σ]. The electric ﬁeld E is an external action applied to the material, and it can be varied at will. It is a ﬁeld tensor. The same applies to the current density, which varies as E varies. On the other hand, the conductivity [σ] does not vary when the ﬁeld E varies. It characterizes a physical property of the crystal, the electrical conductivity: it is called a material tensor because it characterizes the material. Material tensors represent physical properties of the material. Their form largely depends on the isotropic or anisotropic character of the material. We saw, for example, that the electrical conductivity of a material becomes a scalar when the material is isotropic. Whatever their rank, the number of independent coeﬃcients necessary to deﬁne material tensors depends on the crystal symmetry of the material, as we will see in Sections 9.5.2 and 9.6.

Chapter 9 – Crystal anisotropy and tensors

197

In contrast, ﬁeld tensors are deﬁned in the same way for isotropic and anisotropic materials. We just saw the examples of the electric ﬁeld and of the electrical current density, which are rank-1 tensor. We will deﬁne in Chapter 11 the stress tensor and in Chapter 12 the strain tensor: they both are second-rank ﬁeld tensors. In Chapter 13, we will see that these two second-rank ﬁeld tensors are related, in a material, by a material tensor of rank 4 which caracterizes the elastic properties of the material.

9.5. Symmetry properties of tensors 9.5.1. Internal symmetry. Symmetric and antisymmetric tensors A tensor of rank n is symmetric with respect to two of its subscripts if the following relation applies: Tab...kl...n = Tab...lk...n . A tensor of rank n is antisymmetric with respect to two of its subscripts if the following relation applies: Tab...kl...n = − Tab...lk...n . Most material tensors have intrinsic symmetry (and, more rarely, antisymmetry) properties which result from thermodynamic considerations, independent of the nature of the crystal. They are called internal symmetry properties. On the other hand, some ﬁeld tensors also feature an internal symmetry, like the stress tensor whose symmetry is related to the balance condition for the solid to which it is applied (Sect. 11.4).

9.5.2. External symmetry of material tensors. Curie’s and Neumann’s principles The inﬂuence of crystal symmetry on material tensors can be described as a direct consequence of Curie’s principle. This principle was stated in 1894 by Pierre and Jacques Curie when studying piezoelectricity, which they had discovered in 1880. It is expressed as follows: When certain causes produce certain eﬀects, the symmetry elements of the causes must be present in the eﬀects. In the same way, when some eﬀects reveal some dissymetry, this dissymetry must be present in the causes which produce them. Consider once more an electric ﬁeld E applied to a material, and the current density j which results because of the electrical conductivity of the material [σ]: j = [σ]E. The causes here are the electric ﬁeld (a polar vector with symmetry ∞ m as shown by Fig. 9.2) and the crystal, with point group Gp (we saw in Sect. 9.2 that the group to be considered in discussing macroscopic properties is

198

Symmetry and Physical Properties of Crystals

the point group of the crystal). The eﬀect is the current density (a polar vector with symmetry ∞ m). Thus the symmetry of the causes is the intersection ∞ m ∩ Gp of the two point groups, which must be less than or equal to the symmetry of the current density ∞ m. The symmetry of the causes here depends on the symmetry of the crystal and on the orientation of the electric ﬁeld with respect to the symmetry elements of the crystal. In the most general case, when the electric ﬁeld has a general direction with respect to the symmetry elements of the crystal, there is no symmetry element common to the crystal and the electric ﬁeld. The symmetry ∞ m of the current density is then larger than the intersection ∞ m ∩ Gp , and nothing special can be stated. The interesting cases are those for which there is an intersection between ∞ m and Gp . For example, if Gp contains a q-fold axis and if the electric ﬁeld is parallel to the q-fold axis, then the intersection of the symmetry elements is the q-fold axis. The eﬀect, which must be at least as symmetric, will therefore be a current density parallel to the q-fold axis. Carrying this argument further, and using the properties of rank-2 tensors which we will see in the next chapter, precise information can be gained on the symmetry of the conductivity tensor in relation to the symmetry of the crystal. Curie’s principle is very general. It applies to all areas of physics. For crystallographic applications, one may prefer Neumann’s principle, which is less general and was laid down earlier (1885). It is expressed as follows: The symmetry elements of any macroscopic physical property of a crystal must include the symmetry elements of the point group of the crystal. Expressed diﬀerently, the symmetry group of any physical property of the crystal includes that of the crystal. Thus the point symmetry group of the crystal is either identical to the symmetry group of the physical property, or it is a subgroup of the latter. Consider for an illustration the example of pyroelectricity. Some crystals, called pyroelectrics (see Chap. 15), exhibit a spontaneous electric polarization P. This quantity is diﬃcult to evidence, because the distribution of electric charges which it entails are rapidly neutralized by free charges in air or by migration of charges within the crystal. However, since this polarization varies with temperature, a rapid variation of temperature ΔT entails a rapid variation, ΔP, of the polarization, which in turns produces a current which is easy to detect. ΔP and ΔT are related by: ΔP = pΔT where p is a vector (rank-1 tensor) which represents the property of pyroelectricity in the material. The symmetry group of a polar vector is ∞ m (Fig. 9.2). Therefore, according to Neumann’s principle, the point group of a pyroelectric crystal must be a subgroup of this group. The only possibilities are the groups: 1

2

3

4

6

Chapter 9 – Crystal anisotropy and tensors

199

A

M

Figure 9.2: Symmetry elements of a polar vector: an A∞ axis parallel to the vector, and an inﬁnity of mirrors containing this axis and those obtained by adding to each of these groups a mirror that goes through the n-fold axis, hence the groups m

mm2

3m

4mm

6mm

thus in total 10 point groups. Crystals with one of these 10 point groups can feature pyroelectricity. It is clear that, if the crystal belongs to one of these groups, the spontaneous polarization will be parallel to axis An for all the groups that have one. For group m, it will be parallel to the mirror and for group 1, its direction is not predetermined by symmetry. We just applied Neumann’s principle directly to a vector physical property for which the symmetry (∞ m) is known. It can also be applied to a symmetric second-rank tensor, whose symmetry is that of an ellipsoid, mmm, as we will see in Section 10.5. For higher-rank tensors, it is convenient to use an equivalent form of Neumann’s principle: if a crystal is invariant under a given symmetry operation, all of its physical properties are invariant under this symmetry operation. Imagine the following experiment. We ﬁrst measure a physical property in a given reference system for a given position of the crystal. Then we submit the crystal to one of its point symmetry operations, and we again measure the physical property in the same reference system. The result obtained must be identical to the former one. Since it is equivalent to perform the symmetry operation on the crystal or the inverse operation (necessarily also a member of the group) on the coordinate system, we will retain the second deﬁnition. Thus: To determine the number of independent components of a tensor representing a physical property of a given crystal, it is suﬃcient to express the invariance of the tensor when all the symmetry operations of the crystal’s point group are applied to the coordinate system.

200

Symmetry and Physical Properties of Crystals

It is clearly suﬃcient to consider only those symmetry operations which are generating all the elements of the point group.

9.6. Reduction in the number of independent coeﬃcients of a material tensor We present two methods for reducing the number of components of a tensor, both using the invariance property stated above.

9.6.1. Method using the transformation matrix We apply the very deﬁnition of a tensor based on the transformation of its components in a change of reference frame (Sect. 9.4.1), viz. = ail ajm akn . . .Tlmn... Tijk...

The Tijk... are the coeﬃcients of a tensor expressed in a ﬁrst, general, orthonor are the coeﬃcients of this same tensor expressed in mal frame and the Tijk... another frame, deduced from the former by a symmetry operation of the crystal’s point group. The aij are the coeﬃcients of the transformation matrix from the ﬁrst frame to the second. The invariance of the components of the tensor under this special change in frame implies that = Tijk.... Tijk...

As an example, we consider a physical property represented by a secondrank tensor, and examine in turn the case of crystals with point groups 2, m and 2/m. If the point group is 2, we can choose the axis system so that axis Ox2 is parallel to the two-fold axis. A rotation by π around axis Ox2 changes the frame R {e1 , e2 , e3 } into a frame R {e1 , e2 , e3 } such that e1 = −e1 ,

e2 = e2 ,

e3 = −e3 .

The only non-zero coeﬃcients of the frame change matrix A are thus: a11 = −1,

a22 = 1

and

a33 = −1

and we deduce that in this transformation = T11 T11 T12 T21

= −T12 = −T21

T22 = T22 T13 T31

= T13 = T31

T33 = T33

T23 = −T23

T32 = −T32 .

(9.16)

Furthermore, we must have Tij = Tij .

(9.17)

Chapter 9 – Crystal anisotropy and tensors

201

= −T We thus deduce for instance that T12 = 0 since T12 12 from (9.16) and T12 = T12 from (9.17). In the same way, T21 = 0, T23 = 0 and T32 = 0, and the tensor ﬁnally is: ⎛ ⎞ T11 0 T13 ⎝ 0 T22 0 ⎠ (9.18) T31 0 T33

For this representation of the tensor, we use the classical notation of matrices: the ﬁrst subscript designates the row and the second one the column. If the point group is m, we can choose an axis system such that axis Ox2 is perpendicular to the mirror. This mirror operation changes frame R into a frame R such that e1 = e1

e2 = −e2

e3 = e3 .

The non-zero coeﬃcients in the transformation matrix are thus a11 = 1, a22 = −1 and a33 = 1. We easily see that we obtain the same tensor form as above in (9.18). Thus the presence of a two-fold axis or of a mirror perpendicular to this axis reduces the number of components of a second-rank tensor in the same way. The form given in (9.18) is therefore that for a second-rank tensor representing a physical property of a crystal belonging to any one of the point groups 2, m, 2/m (monoclinic groups) when the axis Ox2 is chosen parallel to the 2-fold axis or perpendicular to the mirror.

9.6.2. “Direct inspection” method This method, due to Fumi [4], uses another aspect of the deﬁnition of tensors, viz. the fact that the components of a tensor transform in an axis change like a product of coordinates. We thus consider directly the products of coordinates. Let us apply this method to the example above. A rotation by π of the coordinate system around axis Ox2 changes the coordinates xi of a point M into coordinates xj such that x1 = −x1 ,

x2 = x2 ,

x3 = −x3 .

We immediately deduce that, for a second-rank tensor, only the components that have one subscript, and only one, equal to 2 will be zero since, in these cases, xi xj = −xi xj , whence Tij = −Tij while Tij = Tij . In the same way, the operation of a mirror perpendicular to Ox2 changes the coordinates xi of a point M into coordinates xj such that x1 = x1 ,

x2 = −x2 ,

We thus retrieve the preceding results.

x3 = x3 .

202

Symmetry and Physical Properties of Crystals

This method is easy to apply, and it is the one used in practice for all the symmetry operations for which the new components xi are expressed as functions of a single component xi . This is the case for all symmetry operations associated to 2- and 4-fold axes, to centers of symmetry and to mirrors. For 3and 6-fold axes, the preceding method, using the transformation matrix from one frame to another, is preferred, except for cubic crystals, where the 3-fold axes are parallel to the < 111 > directions. In the latter case, one chooses an orthonormal coordinate system parallel to the basis vectors of the crystal system. A rotation of the coordinate system by 2π/3 around a [111] direction transforms the coordinates xi of a point P into coordinates xi such that x1 = x2 ,

x2 = x3 ,

x3 = x1

and the direct inspection method is easy to use. We note that, in all cases, the reduction in the number of components is performed with an orthonormal axis system in which one axis (or several) is parallel or perpendicular to a symmetry element of the crystal.

9.6.3. Special case: central symmetry (inversion symmetry) In this case both methods are equally convenient. The transformation matrix is such that aij = −δij , and we obtain, for a rank-n tensor = (−1)n Tijk... = Tijk... Tijk...

(9.19)

1.

If n is odd, we conclude that all the tensor’s components are zero. Thus an odd-rank tensor representing a physical property of a crystal has non-zero components only if the crystal has no center of symmetry. We will see that piezoelectricity, which is described by a third-rank tensor, exists only in crystals that do not have a center of symmetry.

2.

If n is even, the tensor is unchanged by the existence of a center of symmetry, and adding a center of symmetry changes nothing to the number of independent coeﬃcients of the tensor. Hence, for the physical properties represented by even-rank tensors, the number of independent coeﬃcients is the same for all point groups of a Laue class (see Sect. 5.7).

We note that relation (9.19) applied to even-rank tensors shows that a central symmetry operation applied to the coordinate system in which the tensor components are expressed leaves its components invariant. This property can be considered without any reference to a crystal. It is general, and the property obtained is therefore also valid for ﬁeld tensors. We can thus state this result in the following form: a central symmetry operation applied to any even-rank tensor (be it a ﬁeld tensor or a material tensor) leaves this tensor invariant.

Chapter 9 – Crystal anisotropy and tensors

203

9.7. Exercises Exercise 9.1 Consider a symmetrical rank-2 material tensor [T ] representing a physical property of a crystal with point group 3. Let Tij be the components of this tensor in an orthonormal axis system (Ox1 x2 x3 ) where Ox3 is parallel to the 3-fold axis. 1.

Let (Ox1 x2 x3 ) be an axis system deduced from (Ox1 x2 x3 ) through a rotation by 2π/3 around axis Ox3 . Determine the transformation matrix {aij } from axis system (Ox1 x2 x3 ) to axis system (Ox1 x2 x3 ).

2.

, T and T of [T ] in the axis system (Ox x x ), Express the components T11 12 22 1 2 3 and deduce that T11 = T22 and T12 = 0.

3.

, T and T , and show that T Calculate T13 13 = T23 = 0 and T33 = 0. 23 33

Exercise 9.2 Use the direct inspection method to determine the number of non-zero coefﬁcients for a material rank-2 tensor of a crystal with point group mmm if its components are expressed in a frame with axes perpendicular to the mirrors.

204

Symmetry and Physical Properties of Crystals

References [1] J.L. Spain, in Chemistry and Physics of Carbon, vol. 8, ed. by P.L. Walker (Marcel Dekker Publisher, New York, 1973), pp. 130–131 [2] D.E. Sands, Vectors and Tensors in Crystallography (Dover Publications, Mineola, New York, 1995) [3] L. Schwartz, Les tenseurs (Hermann, Paris, 1975) [4] F.G. Fumi, Physical properties of crystals: the direct inspection method, Acta Crystallographica 5, 44–48 (1952)

Chapter 10

Second-rank tensors This chapter is devoted to the study of the characteristic properties of symmetric tensors of rank 2. They represent many physical properties which, in isotropic materials, are described by a simple scalar. The end of this chapter introduces axial vectors, which are antisymmetric tensors of rank 2, and gives examples.

10.1. Introduction Second-rank tensors are very important in physics. Because most of them are symmetric, it is useful to investigate their special properties, and in particular the quadric which is associated to them (Sect. 10.2, 10.3 and 10.4). Section 10.5 investigates the eﬀect of crystal symmetry on material tensors of rank 2. Section 10.6 deﬁnes axial vectors, and shows that they are antisymmetric tensors of rank 2.

10.1.1. Symmetric and antisymmetric tensors A second-rank tensor is symmetric if Tij = Tji whatever i and j, and the matrix which represents it in a general axis system has the form ⎞ ⎛ T11 T12 T13 ⎝ T12 T22 T23 ⎠ . T13 T23 T33 There are thus 6 independent coeﬃcients. A second-rank tensor is antisymmetric if Tij = −Tji , hence T11 = T22 = T33 = 0, so that, in matrix representation: ⎞ ⎛ 0 T12 T13 ⎝ −T12 0 T23 ⎠ . −T13 −T23 0 There are thus 3 independent coeﬃcients.

© Springer Science+Business Media Dordrecht 2014 C. Malgrange et al., Symmetry and Physical Properties of Crystals, DOI 10.1007/978-94-017-8993-6_10

205

206

Symmetry and Physical Properties of Crystals

Any second-rank tensor [T ] can be written as the sum of a symmetric tensor [S] and an antisymmetric tensor [A]: [T ] = [S] + [A], with Tij + Tji 2 Tij − Tji . Aij = 2 Sij =

and

This decomposition is independent of the frame in which tensor [T ] is expressed. We demonstrate this for the symmetric part. In another orthonormal axis of tensor [S] become S = a a S system (Ox1 x2 x3 ), the components Sij ik jl kl ij = S . (Eq. (9.13a)). If Skl = Slk , it is clear that Sij ji

10.1.2. Matrix form of second-rank tensors We saw that it is customary to represent the components of a rank-2 tensor, in a given system of axes, by a matrix, extending to tensors the usual rule for writing matrices. Thus the component Tkl of the tensor is at the intersection of the k-th row and the l-th column of matrix T . In another system of axes, deduced from the ﬁrst one through the transformation matrix A, the new takes the form component Tkl = aki alj Tij . Tkl

If AT is the transposed matrix of A, aTij = aji and = aki Tij aTjl Tkl

so that, in matrix notation T = AT AT .

(10.1)

10.1.3. Trace The trace of a second-rank tensor [T ], represented in a given system of axes, is deﬁned by: Tr [T ] = T11 + T22 + T33 = Tii . It is independent of the referential chosen to represent the tensor. The trace of tensor [T ] in a new axis system, Tr ([T ]) , is expressed, using relation (9.13a), by: (Tr [T ]) = Tii = aik ail Tkl . From (9.10): aik ail = δkl and (Tr [T ]) = δkl Tkl = Tkk . Hence (Tr [T ]) = Tr [T ].

Chapter 10 – Second-rank tensors

207

10.2. Representative quadric for a symmetric rank-2 tensor 10.2.1. Characteristic surface Consider the following equation: Sij xi xj = ±1 = ε

(10.2)

where, for the moment, the coeﬃcients Sij are general, but satisfy the condition Sij = Sji . When expanded, this equation takes the form S11 x21 + S22 x22 + S33 x23 + 2S12 x1 x2 + 2S13 x1 x3 + 2S23 x2 x3 = ε.

(10.3)

The locus of the points M with coordinates x1 , x2 , x3 in an orthonormal frame is a second-degree surface, also called quadric (Q) (an ellipsoid or a hyperboloid), having for its center the coordinate origin O. We want the equation of this quadric in another frame (Ox1 x2 x3 ) obtained from (Ox1 x2 x3 ) through the transformation matrix A = {aij }. xi = aki xk

From Equation (9.9): and Equation (10.2) becomes:

Sij aki xk alj xl = ε x x = ε if S = a a S . which can be written as: Skl ki lj ij k l kl

Thus the coeﬃcients Sij which deﬁne the quadric (Q) transform in a change of orthonormal frame like the components of a second-rank tensor. If the coeﬃcients Sij in Equation (10.2) are the coeﬃcients of a symmetric tensor, the quadric (Q) is a geometrical representation of this tensor. We have thus deﬁned the representation quadric of a symmetric tensor [S].

10.2.2. Principal axes and principal coeﬃcients The quadrics (ellipsoids or hyperboloids on Fig. 10.1) have as symmetry elements three mutually perpendicular mirrors, three 2-fold axes at the intersections of these mirrors, and a center of symmetry. In an orthonormal set of axes (Ox1 x2 x3 ) parallel to these 2-fold axes, called the principal axes of the quadric, the equation of the quadric becomes: (x1 )2 + S22 (x2 )2 + S33 (x3 )2 = ε. S11

(10.4)

In this new system of axes, called the principal axes of the tensor, the tensor takes a diagonal form: ⎞ ⎛ 0 S11 0 ⎝ 0 S22 0 ⎠ 0 0 S33

208

Symmetry and Physical Properties of Crystals x3

x3

x2 x1

(a)

(b)

x3

x3

(c)

(d)

Figure 10.1: Representation quadrics of a symmetric second-rank tensor: (a) an ellipsoid, if the three principal values have the same sign; (b) onesheeted hyperboloid; (c) two-sheeted hyperboloid; (d) the set of two hyperboloids representing the tensor when one of the principal values has a sign opposite to the two others , S and S are called the principal values or the principal coeﬃcients and S11 22 33 of tensor [S].

To determine these principal axes (of the quadric and of the tensor), we note that, along these special directions, the normal to the quadric is parallel to the radius vector of the quadric. We know that, if the equation of a surface is f (x1 , x2 , x3 ) = 0, the components Xi of a vector perpendicular to this surface are Xi = ∂f /∂xi . A vector normal to the quadric with Equation (10.3) thus has for its components Xi at a point with coordinates xj : Xi = 2Sij xj . It is parallel to the radius vector with components xi if: Sij xj = λxi

(10.5)

Chapter 10 – Second-rank tensors

209

where λ is any scalar. This system of three equations is just the tool needed to determine the eigenvectors and eigenvalues of matrix {Sij }. Since this matrix is real and symmetric, it has three real and orthogonal eigenvectors, the eigenvalues of which are real. We can thus determine the directions of the symmetry axes of the quadric; they coincide with the principal axes of the tensor.

10.2.3. Shape of the quadric In the frame (Ox1 x2 x3 ) of its principal axes, the quadric is deﬁned by the three , S and S . Its geometrical shape depends on the signs of coeﬃcients S11 22 33 these three coeﬃcients. , S and S are positive, we choose ε = 1, and the equation of the If S11 22 33 quadric can be expressed in the form:

x12 x22 x32 + 2 + 2 = 1, a2 b c the equation of an ellipsoid (Fig. 10.1a) with semi-axes a, b and c such that: 1 b= , S22

1 a= , S11

1 c= . S33

The principal values of the tensor are thus the reciprocals of the squares of the semi-axes of the ellipsoid. , S and S are negative, the associated quadric would be an imaginary If S11 22 33 ellipsoid if ε was chosen as equal to 1. We choose ε = −1 so that the quadric is an ellipsoid. The principal values of the tensor are negative, and their absolute values are the reciprocals of the squares of the semi-axes of the ellipsoid. < 0), If two coeﬃcients are positive and the third one negative (for example S33 and if we choose ε = 1, the equation of the quadric has the form:

x12 x22 x32 + 2 − 2 = 1, a2 b c with a2 =

1 , S11

b2 =

1 , S22

c2 = −

1 . S33

This is the equation of a one-sheet hyperboloid (Fig. 10.1b). The sections of this hyperboloid by the planes x3 = const are ellipses, while the sections by the planes x1 = const and x2 = const are hyperbolas. If we choose ε = −1, the equation becomes:

−

x12 x22 x32 − 2 + 2 =1 a2 b c

and the quadric is a two-sheeted hyperboloid (Fig. 10.1c). In order to obtain a representation of the tensor in all directions of space, the representation

210

Symmetry and Physical Properties of Crystals

quadric of the tensor consists of the two hyperboloids tangent to the same cone, whose apex is the origin of the axes (Fig. 10.1d). > 0), If two coeﬃcients are negative and the third one positive (for example S33 we retrieve the preceding case if we set:

a2 = −

1 , S11

b2 = −

1 , S22

c2 =

1 . S33

The one-sheet hyperboloid is obtained with ε = −1 and the two-sheeted one with ε = 1. We will see an application in Section 12.6. In practice, the principal values of a tensor are usually all positive, and the quadric is then an ellipsoid, the equation of which is given by (10.4) with ε = 1. This is, for simplicity, what we will assume in the next section.

10.3. Properties of the quadric Consider a second-rank tensor [T ] which relates vector A to vector B through relation B = [T ]A, i.e. Bi = Tij Aj . We will, to simplify the presentation, call vector A the cause and vector B the eﬀect even if tensor [T ] is a ﬁeld tensor for which this denomination is not justiﬁed.

10.3.1. Normal to the quadric We saw (Eq. (10.5)) that the normal to point M (x1 , x2 , x3 ) of the quadric Tij xi xj = 1 is a vector with components Xi = 2Tij xj , i.e. a vector parallel to the vector [T ]OM with components Tij xj . We deduce that, if the cause vector is parallel to radius vector OM, the associated eﬀect vector is parallel to the normal to the quadric at point M. Figure 10.2 illustrates this result. We chose the electric ﬁeld E as the cause vector, and its eﬀect is the current density j, which is related to it by the electrical conductivity [σ]: j = [σ]E. x2

j E s

O

M x1

Figure 10.2: If the direction of the cause vector (electric ﬁeld E) is along OM, the eﬀect vector (electric current density j) is along the normal at point M to the quadric representing the electrical conductivity tensor.

Chapter 10 – Second-rank tensors

211

10.3.2. Length and physical meaning of the radius vector Let M be a point of the quadric representing tensor [T ] which connects cause vector A to eﬀect vector B through relation B = [T ]A. Set: OM = rs where s is a unit vector. We deduce: xi = rsi . The equation of quadric Tij xi xj = 1 becomes: Tij r 2 si sj = 1 so that

1 = si Tij sj r2

which can be written in matrix form: ⎛ ⎞⎛ ⎞ T11 T12 T13 s1 1 = s1 s2 s3 ⎝ T12 T22 T23 ⎠ ⎝ s2 ⎠ . r2 T13 T23 T33 s3

(10.6)

(10.7)

If the cause vector A, with norm A, is parallel to OM, we have A = As, i.e. Aj = Asj . The components Bi of the eﬀect vector are given by: Bi = Tij Aj = Tij sj A and the component of B parallel to A, i.e. B · s, becomes:

1 B · s = Bi si = si Tij sj A = A 2 . r

(10.8)

We deduce that, for a cause vector with unit norm (A = 1), parallel to a given radius vector of the quadric, the reciprocal of the square of the length of this radius vector is equal to the projection of the corresponding eﬀect vector on the direction of the cause vector.

10.3.3. Intensity of a physical property in a given direction If tensor Tij is a material tensor representing a given physical property, si sj Tij represents the value of this physical quantity in direction s. We demonstrate this by taking the example of electrical conductivity [σ], with components σij in a given axis system. A measurement of the conductivity of a crystal can be performed by using a parallel-faced plate of this crystal, with thickness e small with respect to the sides of the main face. A voltage V is applied between the metallized major faces. It induces, except for edge eﬀects which we neglect, an electric ﬁeld E perpendicular to the plate, so that E = Es where s is a unit

212

Symmetry and Physical Properties of Crystals

vector perpendicular to the plate and E = V /e. We then measure the intensity in the circuit, and deduce the current density (the intensity of the current in the circuit, divided by the area of the crystal perpendicular to the electric ﬁeld, hence in this case the area of the major faces). The latter is the component js of the current density along the normal s to the crystal (Fig. 10.3), so that: js = j · s = ji si = σij sj si E.

j

s

js

E

V

Figure 10.3: Schematic diagram of the principle of the experimental device for measuring the electrical conductivity of a crystal plate, the major faces of which were metallized The conductivity in direction s is deﬁned as the quantity σs such that: σs =

js = σij si sj . E

In a general way, the value Ts in a direction with unit vector s of a physical property represented by tensor [T ] is given by si sj Tij . From (10.6), Ts =

and

1 r2

1 r= √ . Ts

(10.9)

Knowing the length of the radius vector OM of the quadric thus provides the value of the physical property in direction OM.

Chapter 10 – Second-rank tensors

213

10.4. Geometrical determination of the principal axes and principal coeﬃcients: the Mohr circle construction We just saw that a symmetric tensor [T ] its principal axes (Ox1 x2 x3 ): ⎛ T11 0 T = ⎝ 0 T22 0 0

can be written in the referential of ⎞ 0 0 ⎠. T33

Consider a new axis system (Ox1 x2 x3 ) deduced from (Ox1 x2 x3 ) through rotation by angle θ around Ox3 . In this new axis system, the components Tij of [T ] are expressed as: Tij = aik ajl Tkl where the transformation matrix A = {aij } is: ⎛ ⎞ cos θ sin θ 0 A = ⎝ − sin θ cos θ 0⎠ . 0 0 1 We obtain:

= a1k a1l Tkl = a11 a11 T11 + a12 a12 T22 + a13 a13 T33 , T11 = cos2 θ T11 + sin2 θ T22 , T11

T22 = a2k a2l Tkl = a21 a21 T11 + a22 a22 T22 + a23 a23 T33 ,

= sin2 θ T11 + cos2 θ T22 , T22 = T33 . T33

In the same way:

= 0, T13

= 0, T32

= T21 = − sin θ cos θ T11 + sin θ cos θ T22 . T12

Thus, tensor [T ] is expressed, in the frame (Ox1 x2 x3 ), as: ⎞ ⎛ 0 T11 T12 ⎝ T12 T22 0 ⎠. 0 0 T33 , T and T as a function of cos 2θ and sin 2θ: We now express T11 22 12

1 1 (T11 + T22 ) − (T22 − T11 ) cos 2θ 2 2 1 1 = (T11 + T22 ) + (T22 − T11 ) cos 2θ 2 2 1 = (T22 − T11 ) sin 2θ. 2

= T11 T22 T12

(10.10)

214

Symmetry and Physical Properties of Crystals

The set of relations (10.10) can be expressed graphically by using the Mohr circle representation (Fig. 10.4). Points A and B are placed along axis Ox1 so that OA = T11 and OB = T22 . We draw circle C, with its center C at the middle of segment AB, and with diameter d equal to the norm of AB. Relations (10.10) become: AB cos 2θ, 2 AB cos 2θ, = OC + 2 AB = sin 2θ. 2

= OC − T11 T22 T12

We draw the axis Cx2 such that angle (Cx1 , Cx2 ) is equal to π/2, then the radius CP of circle C enclosing angle 2θ with axis Ox1 . Let P be the point diametrically opposite to P. Let H and J be the respective projections of P and = OH, P on axis Cx1 , and K the projection of P on axis Cx2 . We see that: T11 T22 = OJ and T12 = CK. x2

C

O

T11 A

T’11 H

T’12 K

P 2 T’22

C

J

T22 B

x1

P’

Figure 10.4: Mohr circle construction This construction makes it possible to easily determine how the tensor coeﬃcients vary when the coordinate axes are rotated. Furthermore, this construction, when performed the other way, makes it possible to quickly determine the principal axes of a second-rank tensor for which only one principal axis is known. The procedure that provides the principal axes and principal values of a tensor which, expressed in its initial frame, has the form: ⎛ ⎞ T11 T12 0 ⎝ T12 T22 0 ⎠ 0 0 T33

Chapter 10 – Second-rank tensors

215

is given below, where ψ is the angle by which we must rotate the initial frame around axis Ox3 to obtain the diagonal form (the angle opposite to the preceding angle θ), and T11 and T22 are the principal values associated to axes Ox1 and Ox2 respectively. and OJ = T . Let Points H and J are placed on axis Ox1 so that OH = T11 22 C be the middle of HJ. Point K is placed on axis Cx2 , perpendicular to Ox1 , . Points J and K deﬁne respectively the abscissa and the so that CK = T12 ordinate of a point P in the axis system (Cx1 , Cx2 ). Angle 2ψ is then the angle (CP, Cx1 ). Let R be the length of vector CP. We obtain T11 = OC − R and T22 = OC + R.

Notes: 1.

It is evident that, if angle 2ψ is larger than π, it will be simpler to choose an angle equal to 2ψ − π, i.e. a rotation angle ψ − π/2, and to interchange T11 and T22 .

2.

If the subspace to be diagonalized is (Ox1 , Ox3 ), then axis Ox1 will be substituted by Ox3 and axis Ox2 by Ox1 in the above construction.

10.5. Eﬀect of crystal symmetry To determine the number of independent coeﬃcients of a symmetric secondrank material tensor (a tensor representing a physical property of a crystal), we can use either of the methods presented in Sections 9.6.1 and 9.6.2. A more elegant and quicker method consists in using the representative quadric of the tensor: according to Neumann’s principle, it must be at least as symmetric as the crystal. The symmetry elements of a general quadric are: one symmetry center, three A2 axes, which are the principal axes, three mirrors perpendicular to the A2 axes. Hence the point group of the quadric is mmm. We deduce for example that: if the crystal has a 2-fold axis, one of the principal axes of the quadric is necessarily parallel to this 2-fold axis. if the crystal has an axis with order n larger than 2 (n = 3, 4 or 6), the quadric must also have an axis with order larger than 2. For a quadric, this can only be an axis of revolution (the symmetry of a revolution quadric is ∞/mm). This axis of revolution is then parallel to the n-fold axis.

216

Symmetry and Physical Properties of Crystals

We now apply these results to the various crystal groups, assuming for simplicity that the representation quadric of the tensor is an ellipsoid. This assumption does not aﬀect the generality of the results to be obtained. We will also see that, ﬁnally, the number of independent coeﬃcients of a symmetric second-rank tensor is the same for all the groups of a given crystal system.

10.5.1. Triclinic system A crystal with point group 1 has no symmetry element. The directions of the principal axes of the quadric then have no special connection with those of the basis vectors a, b and c of the crystal. The tensor representing the physical property of this crystal then has 6 independent coeﬃcients. If the point group of the crystal is ¯1, the result is the same since the quadric has a center of symmetry. This result is no surprise since we showed (Sect. 9.6.3) that even-rank tensors are invariant under a central symmetry operation. The tensor has the most general form: ⎞ ⎛ T11 T12 T13 ⎝ T12 T22 T23 ⎠ . T13 T23 T33 Its principal axes can now be determined. The six independent coeﬃcients are retrieved: the three principal values, and the three parameters which deﬁne the orientation, with respect to the crystal itself, i.e. with respect to the basis vectors of its unit cell, of the orthonormal trihedron parallel to the principal axes.

10.5.2. Monoclinic system Such a crystal has at least a 2-fold axis (group 2) or a mirror (group m). One of these symmetry elements therefore necessarily coincides with one of the symmetry elements of the ellipsoid. If an orthonormal axis system is chosen so that axis Ox3 be parallel to axis A2 , or perpendicular to mirror m, the tensor takes the form: ⎞ ⎛ T11 T12 0 ⎝ T12 T22 0 ⎠ . 0 0 T33 If the crystal group is 2/m, the same result is obtained, since the quadric has a mirror perpendicular to each of the A2 axes. We retrieve the result of the example discussed in Section 9.6.1, except that we here chose axis Ox3 parallel to the 2-fold axis and perpendicular to the mirror.

10.5.3. Orthorhombic system In this system, a crystal has at least three mutually orthogonal 2-fold axes (group 222) or two mutually orthogonal mirrors (group mm2). These symme-

Chapter 10 – Second-rank tensors

217

try elements must be common to the crystal and to the ellipsoid representing the physical property. The axes of the ellipsoid are therefore parallel to the basis vectors of the orthorhombic unit cell: thus the orientation of the ellipsoid is ﬁxed. In a system of orthonormal axes parallel to the basis vectors a, b and c, the tensor has the form: ⎛ ⎞ T11 0 0 ⎝ 0 T22 0 ⎠ . 0 0 T33 This result is valid also for group mmm, which is the symmetry group of the ellipsoid.

10.5.4. Uniaxial systems: rhombohedral, trigonal and hexagonal A crystal belonging to any one of these systems has at least one n-fold axis, with n larger than 2 (except for groups ¯4 and ¯ 42m). The same must apply to the ellipsoid, which is therefore of revolution around this axis. If Ox3 is chosen parallel to axis An , the tensor has the form: ⎞ ⎛ 0 T11 0 ⎝ 0 T11 0 ⎠ . 0 0 T33 The additional symmetry elements in any of these crystal groups do not contribute additional relations among the coeﬃcients, because the ellipsoid already has all the symmetry elements which can be added. The same result is obtained for groups ¯4 and ¯42m, for example using the direct inspection method (Exercise 10.4) or, alternatively, by noting that the number of independent coeﬃcients for even-rank material tensors is the same for all groups in a given Laue class (Sect. 9.6.3).

10.5.5. Cubic system All groups in this crystal system have four A3 axes. The only ellipsoid compatible with the presence of four A3 axes is a sphere. The quadric is therefore a sphere. The tensor is diagonal, with its three coeﬃcients equal: ⎛ ⎞ T 0 0 ⎝ 0 T 0 ⎠ 0 0 T whatever the axis system in which it is represented. We conclude that: The physical properties represented by a rank-2 tensor are isotropic in a cubic crystal.

218

Symmetry and Physical Properties of Crystals

10.6. Axial vectors, or antisymmetric rank-2 tensors 10.6.1. Polar vectors, axial vectors Two families of vector-type physical quantities must be distinguished: the quantities obviously represented by vectors (displacement, velocity, acceleration, force. . . ): these are called polar vectors. the quantities which describe a rotation, such as angular velocity, the moment of a force, magnetic ﬁeld. . . These are called axial vectors.

They are denoted as V and represented by a line and a sense of rotation around this line. It is however convenient to also represent them through vectors. This requires choosing a convention to connect the direction of the vector and the sense of rotation. The convention chosen is the following: the vector points so that the rotation associated to the axial vector be, for this vector, in the direct direction (Fig. 10.5).

Figure 10.5: Convention for representing axial vectors through vectors These two vector families transform diﬀerently under some symmetry operations. If an axial vector is submitted to a rotation, the sense of rotation of the axial vector is conserved. Therefore a polar vector and an axial vector transform the same way in a rotation operation. In contrast, the behavior is diﬀerent for symmetry with respect to a center and with respect to a plane. Consider a given vector OP, representing ﬁrst a polar vector, and then an axial vector, using the above convention. Let x1 , x2 and x3 be the components of vector OP in a given orthonormal axis system, and let x1 , x2 and x3 be those of vector OP , the transform of OP in the symmetry operation. Consider ﬁrst the operation corresponding to symmetry with respect to plane (Ox1 , Ox2 ). The components of the polar vector OP are (Fig. 10.6a): x1 = x1 ,

x2 = x2 ,

x3 = −x3 .

Those of the axial vector OP are (Fig. 10.6b and c): x1 = −x1 ,

x2 = −x2 ,

x3 = x3 .

Now consider the operation corresponding to symmetry with respect to point O. The components of the polar vector OP are (Fig. 10.7a): x1 = −x1 ,

x2 = −x2 ,

x3 = −x3 .

Chapter 10 – Second-rank tensors

219 x3

P

O

x2

x1

(a)

P’

x3

x3

P’

P

O x2

x1

x1

(b)

x2

O

(c)

Figure 10.6: Transformation of polar and axial vectors through symmetry with respect to plane (Ox 1 , Ox 2 ): (a) polar vector; (b) axial vector; (c) polar vectors associated to the axial vectors of Figure (b) x3

P

O x2

x1

(a) x3

x3 P P’

O x2

x1

(b)

x1

O

x2

(c)

Figure 10.7: Transformation of polar and axial vectors through symmetry with respect to point O: (a) polar vector; (b) axial vector; (c) polar vectors associated to the axial vectors of Figure (b)

220

Symmetry and Physical Properties of Crystals

and those of the axial vector OP are (Fig. 10.7b and c) x1 = x1 ,

x2 = x2 ,

x3 = x3 .

The polar and axial vectors thus transform the same way in direct isometries (rotation), and diﬀerently in indirect isometries (symmetry with respect to a plane and central symmetry). This diﬀerence is also encountered when performing a change in coordinate system, since transforming a vector through a symmetry operation is equivalent to performing the inverse symmetry operation on the coordinate system. In a rotation of the coordinate system (direct isometry), the components of a polar vector and of an axial vector transform the same way: from relation (9.8): xi = aij xj

(10.11)

where the xi are the old components, the xi the new components and {aij } is the transformation matrix for going from the old coordinate system to the new system. In contrast, if the coordinate system is submitted to a symmetry with respect to a plane or a central symmetry, which are indirect isometries, it can be checked that the new components xi of the axial vector are expressed as a function of the old ones xi through relation: xi = −aij xj .

(10.12)

Further, since the determinant Δ of matrix {aij } is equal to +1 for direct symmetry operations and to −1 for indirect symmetry operations, we can, for axial vectors, collect relations (10.11) and (10.12) into a single relation: xi = Δaij xj

(10.13)

where Δ is the determinant of the transformation matrix from the old to the new system.

10.6.2. Example of an axial vector: the cross product

Consider a cross product: W = P×Q where P and Q are two polar vectors. It is an axial vector because it is related to the sense of rotation of vector P toward vector Q. It can in fact easily be checked that a central symmetry operation on vectors P and Q transforms vector W into itself. Let p1 , p2 , p3 and q1 , q2 , q3 be the components of P and Q respectively, in an orthonormal axis system (Ox1 x2 x3 ). The components wi of the cross product W = P × Q are:

w1 = p 2 q 3 − p 3 q 2 w2 = p 3 q 1 − p 1 q 3 w3 = p 1 q 2 − p 2 q 1

(10.14)

Chapter 10 – Second-rank tensors

221

which can be written in a condensed form which will prove useful later on: wk = δkij pi qj .

(10.15)

δijk is the Levi-Civita symbol, deﬁned, for any axis

system,1

as:

δijk = 0 if at least two of the subscripts i, j and k are equal, δijk = 1 if the permutation ijk is direct (123, 231, 312), δijk = −1 if it is inverse (132, 213, 321).

Let w1 , w2 , w3 be the components of vector W , the transform of W in a symmetry with respect to the origin. Since a central symmetry changes P into −P and Q into −Q, we immediately see on Equations (10.14) that w1 = w1 , w2 = w2 and w3 = w3 , so that W = W. We can associate the components of W to coeﬃcients Vij deﬁned by:

Vij = pi qj − qi pj for i = j V11 = V22 = V33 = 0.

and

w1 = V23 = −V32 ,

We thus have

w2 = V31 = −V13 ,

(10.16)

w3 = V12 = −V21 . In another axis system (Ox1 x2 x3 ), deduced from the preceding one through the transformation matrix A with coeﬃcients aij , the components of vectors P and Q become: pi = aij pj

and

qi = aij qj .

The coeﬃcients Vij become, in this new axis system, Vij such that: Vij = pi qj − qi pj = aik pk ajl ql − ain qn ajm pm = aik ajl (pk ql − qk pl ) = aik ajl Vkl . This shows that Vij is a second-rank tensor. Furthermore, it is antisymmetric since Vij = −Vji . Hence: The components of a cross product (an axial vector or an axial tensor 2 of rank 1) are the components of the polar second-rank antisymmetric tensor [V ] deﬁned above.

The axial vector W with components wk and the antisymmetric tensor [V ] deduce from each other through relations: 1 and Vij = δijk wk (10.17) wk = δkij Vij 2 as can be checked easily. 1. We will show in Appendix 18A that this symbol is a rank-3 axial tensor, also called the permutation tensor. 2. The general deﬁnition of an axial tensor is given in Appendix 18A.

222

Symmetry and Physical Properties of Crystals

10.7. Exercises Exercise 10.1 Consider a monoclinic crystal with point group 2, where the basis vector b of the unit cell is perpendicular to the vectors a and c, and a rank-2 symmetric tensor [T ] representing a physical property of this crystal. The components Tij of this tensor, in an orthonormal axis system (Ox1 x2 x3 ) where axis Ox2 is parallel to b, are T11 = 1, T22 = 2, T33 = 3, T13 = T31 = 4 and the other components are zero. 1.

Calculate the components Tij of this tensor in an axis system (Ox1 x2 x3 ) deduced from (Ox1 x2 x3 ) through a rotation by π around Ox3 .

2.

Calculate the components Tij of the same tensor in an axis system (Ox1 x2 x3 ) deduced from (Ox1 x2 x3 ) through a rotation by π around axis Ox2 .

Exercise 10.2 Consider a monoclinic crystal. Its electrical conductivity [σ] is represented in an orthonormal axis system (Ox1 x2 x3 ), where axis Ox2 is parallel to the 2-fold axis, by the following matrix: √ ⎞ ⎛ 7 0 3 ⎝ 0 8 0 ⎠ √ 3 0 5 where the unit is 107 Ω−1 m−1 . 1.

This crystal is submitted to an electric ﬁeld E. Determine the current density vector for the following cases: (a) E is parallel to axis Ox1 , (b) E is parallel to axis Ox2 , (c) E is parallel to axis Ox3 , (d) E is parallel to the bisector of the angle between axes Ox3 and Ox1 , (e) E is in the plane (Ox3 , Ox1 ), and its direction deduces from that of Ox3 through a rotation by 60◦ around Ox2 . What is your conclusion?

2.

A plate with faces parallel to the plane (Ox1 x2 ) is cut out of this crystal, and submitted to an electric ﬁeld E parallel to axis Ox3 . (a) Calculate the component jn of j along the applied ﬁeld (b) What is the meaning of the ratio jn /E, where E is the norm of E?

3.

Express tensor [σ] in a new system of axes, rotated by 60◦ around Ox2 with respect to the preceding one. What do you conclude?

Chapter 10 – Second-rank tensors

223

Exercise 10.3 Let σij be the electrical conductivity tensor of a crystal exhibiting a 3-fold axis. We choose an orthonormal axis system (Ox1 x2 x3 ) such that axis Ox3 is parallel to this axis. 1.

Give the form of this tensor in this axis system.

2.

Calculate the conductivity σs in a general direction, parallel to the unit vector s with direction cosines (s1 , s2 , s3 ). Express it as a function of the non-zero components σij and of the spherical coordinates (r = 1, θ, ϕ) of s. What do you conclude?

Exercise 10.4 1.

Using the direct inspection method, determine the form of a symmetric rank-2 tensor representing a physical property of a crystal with point group ¯4 when it is described in an orthonormal axis system (Ox1 x2 x3 ) in which axis Ox3 is parallel to the ¯4-fold axis and origin O is at the center of symmetry associated with the rotoinversion by π/2.

2.

Now consider a crystal with point group ¯42m, and choose axis Ox1 perpendicular to the mirror. Show that adding this symmetry element does not change the form of the tensor.

Chapter 11

The stress tensor The elastic properties of materials relate the applied stress tensor to the resulting strain tensor via the stiﬀness tensor or its inverse, the compliance tensor. They are the topics of Chapters 11, 12 and 13. In the present chapter, the stress tensor at a point in the material is deﬁned. The basic relations which must be veriﬁed by its spatial derivatives are then determined, and they lead to the condition that this tensor must be symmetric.

11.1. Introduction In Chapters 11, 12 and 13, we investigate the mechanical properties of crystals, i.e. the way they deform under external forces. These external forces induce stresses at each point in the crystal. The relation between the stresses in a material and the external forces applied to its surface is investigated in treatises on the mechanics of continuous media (see for example [1, 2]). Here, we use a few results of mechanics, in particular to locally deﬁne the stress tensor (Chap. 11) and the strain tensor (Chap. 12). At any given point in the crystal, these tensors are related to each other by a material tensor: the compliance tensor, connecting the stress to the strain, or the stiﬀness tensor, connecting conversely the strain to the stress.

11.2. Stress tensor 11.2.1. Introduction In an undeformed solid at equilibrium, each atom or molecule is in an equilibrium position which results from the equality of the attractive and repulsive forces exerted on each of them by the neighboring atoms or molecules (Chap. 8). If the solid is submitted to external forces, it deforms. The external forces are transmitted from atom to atom. Each atom (or molecule) is thus submitted to an additional force, which displaces it to a position where, in the new

© Springer Science+Business Media Dordrecht 2014 C. Malgrange et al., Symmetry and Physical Properties of Crystals, DOI 10.1007/978-94-017-8993-6_11

225

226

Symmetry and Physical Properties of Crystals

equilibrium state, this force is balanced by a restoring force which tends to return the atom or molecule to its initial position. The solid is said to be submitted to stress. Since we are interested in macroscopic properties of the solid, we do not consider an atom but a small volume Δv of the solid, bounded by its surface S (Fig. 11.1). The stresses then lead to forces which the surrounding solid exerts on volume Δv through all elements dS of surface S. More precisely, the solid around Δv exerts on each element dS a force which is proportional to the value of dS: dF = T(r, n)dS. r is the radius vector to the center P of dS : r = O P, and n a unit vector perpendicular to dS, oriented from within Δv to the outside. T(r, n) is a force per unit surface, called the stress at point r; it normally depends not only on r but also on the orientation, deﬁned by n, of the surface on which it acts.

n P dS v S r O’ V

Figure 11.1: Schematic diagram illustrating the surface forces acting on a volume element Δv For a given elementary surface dS, we can consider the material on one side or the other side of the surface. If the normal is oriented from part 1 toward part 2, i.e. if it corresponds to n1 on Figure 11.2, then T(r, n1 )dS represents the force dF2/1 exerted by part 2 on part 1 of the solid. Conversely, for the opposite normal n2 = −n1 , we have T(r, n2 )dS = dF1/2 , which represents the force exerted by part 1 on part 2. The action-reaction law (Newton’s third law) requires these two forces to be equal and opposite: dF1/2 = −dF2/1 We set n1 = n and

and

T(r, n2 )dS = −T(r, n1 )dS.

T(r, n) = −T(r, −n).

The force per unit area T(r, n) is designated as the stress exerted across the small surface element dS, centered at point P such that O P = r, with normal unit vector n, by the part of the solid located on the side toward which vector n is pointing onto the other part. To make the notations simpler, T(r, n) is

Chapter 11 – The stress tensor

227

n1

dF½

dS

dS

dF²⁄1

n2

Figure 11.2: Forces acting on a surface element dS of a solid written as Tn , and it is enough to designate the point P at the center of the small surface element. The volume element Δv can also be submitted to forces proportional to its volume, which will be generally noted fΔv. The simplest example of such a bulk force is the gravity force, equal to ρgΔv where ρ is the mass per unit volume of the solid and g the acceleration of gravity.

11.2.2. Deﬁnition of the stress tensor Consider again the small plane surface element dS centered at P, and its normal vector n. Choose an orthonormal system of axes (Ox1 x2 x3 ) whose origin is located at point O very near dS, and on the side opposite to n (Fig. 11.3). Surface dS intersects axes Ox1 , Ox2 and Ox3 at A, B and C respectively. We thus deﬁne a small tetrahedron, formed by surface ABC and three faces OBC, OCA and OAB respectively perpendicular to Ox1 , Ox2 and Ox3 (Fig. 11.3). x3 TnS(ABC)

C

–T1S(OBC) n

– T2S(OAC) O A

B

x2

– T3S(OAB)

x1

Figure 11.3: Forces acting on the tetrahedron OABC This tetrahedron, with volume Δv, is submitted, through its four faces, to forces related to the stresses deﬁned above, exerted upon it by the part of the solid which is outside. It can also be submitted to bulk forces f Δv. Since this tetrahedron is at equilibrium, the resultant of these forces is zero. The force acting on surface ABC is Tn S(ABC) , in accordance with the deﬁnition of Tn given above.

228

Symmetry and Physical Properties of Crystals

The forces acting on the other faces of the tetrahedron are: on OBC: – T1 S(OBC) , on OCA: – T2 S(OCA) , on OAB: – T3 S(OAB) . Here, we call by convention Ti the stress acting on a surface normal to axis Oxi , with its normal oriented toward the positive Oxi (in other words, the stress exerted by the solid lying on the positive xi side onto the solid lying on the negative xi side). In the case of the forces applied by the surrounding medium upon tetrahedron OABC, the normals to the surfaces OBC, OAC and OAB are oriented respectively toward the negative Ox1 , Ox2 , Ox3 . This explains the minus signs. The equilibrium condition for the tetrahedron is given by: −T1 S(OBC) − T2 S(OCA) − T3 S(OAB) + Tn S(ABC) + f Δv = 0.

(11.1)

We now express the areas of triangles OAB, OBC and OCA as a function of the area of triangle ABC. We note that OAB is the projection of area ABC onto plane (Ox1 ,Ox2 ), which is normal to Ox3 , hence S(OAB) = S(ABC) cos(n, Ox3 ) = n3 S(ABC) where we note n1 , n2 , n3 the direction cosines of vector n. In the same way: S(OBC) = S(ABC) cos(n, Ox1 ) = n1 S(ABC) , S(OCA) = S(ABC) cos(n, Ox2 ) = n2 S(ABC) . We can thus write relation (11.1) in the form: Tn S(ABC) − T1 n1 S(ABC) − T2 n2 S(ABC) − T3 n3 S(ABC) + f Δv = 0. Allowing volume Δv to tend to zero, the ratio Δv/S(ABC) tends to zero, and we can write: Tn = n 1 T1 + n 2 T2 + n 3 T3 . Projecting this equation onto the three axes, we obtain (Tn )1 = T11 n1 + T12 n2 + T13 n3 (Tn )2 = T21 n1 + T22 n2 + T23 n3 (Tn )3 = T31 n1 + T32 n2 + T33 n3 where we denote by Tij the component parallel to Oxi of the stress Tj . The three above equations can be written in the following condensed form: (Tn )i = Tij nj

(11.2)

where (Tn )i is the component parallel to Oxi of the stress exerted on the face ABC normal to the unit vector n, with components nj , by the part of the

Chapter 11 – The stress tensor

229

material located on the side toward which n points onto the part located on the other side of ABC. This relation shows that the coeﬃcients Tij relate vector n, normal to face ABC, to the vector Tn representing the stress acting on this face. We saw (Sect. 9.4.2) that, if two vector quantities A and B, with components respectively Ai and Bi , are related by Bi = Tij Aj , then the Tij are the components of a second-rank tensor [T ]. Hence we can write: Tn = [T ]n. The stress tensor [T ] describes an external action which depends, not on the crystal itself, but on the forces which are applied on its surface by the external world. It is a ﬁeld tensor. The component Tij of this tensor is the component parallel to axis Oxi of the force per unit area (the stress) exerted on a surface element normal to Oxj by the part on the positive Oxj side of the solid onto the part located on the negative xj side. Tij component

face

We have deﬁned the tensor Tij at point P as Tij (r). In the special case where Tij does not depend on the position of P in the solid, the stress tensor is said to be uniform.

11.2.3. Normal stress and shear stress The diagonal terms of the stress tensor [T ] represent stresses which are called normal because they are the forces perpendicular to the surfaces. For example, T11 is the component parallel to axis Ox1 of the force acting on a surface normal to Ox1 . A positive value of T11 represents a tensile stress whereas a negative value represents a compressive stress. The non-diagonal terms Tij (with i = j) represent the shear components on these faces. For the same stress tensor, we now express the normal stress Tν and shear stress τ for a general surface dS, with normal n, a unit vector with components n1 , n2 , n3 (Fig. 11.4). The components (Tn )i of the stress force Tn applied to the surface dS are given by relation (11.2), viz. (Tn )i = Tij nj . The normal stress Tν = Tν n is the projection of Tn on n and Tν = n · Tn = ni (Tn )i , Tν = ni nj Tij

230

Symmetry and Physical Properties of Crystals T Tn

dS

n

Figure 11.4: Normal stress Tν and shear stress τ acting on a surface dS, with normal n, submitted to stress Tn which can be written in matrix form: ⎛ Tν = n1 n2 n3 ⎝ Tij

⎞⎛

⎞ n1 ⎠ ⎝ n2 ⎠ . n3

Using result (10.7), we deduce that the normal stress Tν is equal to the reciprocal of the square of the length of the radius vector of the quadric representing the stress tensor. The shear stress τ is the projection of Tn on the surface element dS: τ = Tn − Tν n which can also be written as

τ = n × (Tn × n)

since n × (Tn × n) = (n · n)Tn − (n · Tn )n = Tn − Tν n.

11.3. Basic relation In many cases, the stress tensor is not uniform. It varies from point to point in the solid and is noted Tij (r). We now calculate the resultant of the forces to which a small parallelepiped, with sides parallel to Ox1 , Ox2 and Ox3 respectively equal to Δx1 , Δx2 , Δx3 , is submitted, taking into account the possibility of bulk forces f per unit volume. We start by calculating the algebraic sum of the components of the stress forces parallel to Ox1 , T1i dS (Fig. 11.5). The components acting on the faces perpendicular to Ox1 give: [T11 (x1 + Δx1 ) − T11 (x1 )]Δx2 Δx3 =

∂T11 Δx1 Δx2 Δx3 . ∂x1

Those acting on the faces perpendicular to Ox2 give: [T12 (x2 + Δx2 ) − T12 (x2 )]Δx1 Δx3 =

∂T12 Δx2 Δx1 Δx3 ∂x2

Chapter 11 – The stress tensor

231

x3 T13(x3 +x3)x1x2 –T11(x1)x2x3 x3

–T12(x2 )x1x3 T11(x1+x1)x2x3

T12(x2 +x2)x1x3 x2

–T13(x3)x1x2 x1

x1

x2

Figure 11.5: Components parallel to axis Ox 1 of the non-uniform stress forces acting on the faces of a rectangle parallelepiped with sides Δx 1 , Δx 2 and Δx 3 and those acting on the faces perpendicular to Ox3 give: [T13 (x3 + Δx3 ) − T13 (x3 )]Δx1 Δx2 =

∂T13 Δx3 Δx1 Δx2 ∂x3

hence, in total: ∂T1j Δx1 Δx2 Δx3 . ∂xj The component parallel to Ox1 of the resultant of the bulk forces is f1 Δx1 Δx2 Δx3 . Let F be the ﬁnal resultant of the stress forces and of the bulk forces acting on unit volume of the material. Its component parallel to Ox1 , F1 , is: F1 =

∂T1j + f1 . ∂xj

The same argument applied to the two other components of F makes it possible to ﬁnally write: Fi =

∂Tij + fi . ∂xj

(11.3)

Since the solid is at equilibrium, Fi = 0, and we obtain: ∂Tij + fi = 0. ∂xj

(11.4)

If the bulk forces are negligible with respect to the stresses: ∂Tij = 0. ∂xj

(11.5)

232

Symmetry and Physical Properties of Crystals

Relation (11.3) will be used in Chapter 14 to investigate the propagation of matter displacements (elastic waves). Since the solid is then no more at equilibrium, it will be applied to Newton’s second law. Relation (11.4) can also be derived in a more formal way by writing the equilibrium condition for a volume V of the solid, submitted to bulk forces f per unit volume and to surface forces FS per unit area, represented by tensor [T ]: f dV + dFS = 0, V

or

S

f (r)dV + V

T(r, n)dS = 0. S

which can be rewritten for each component i, taking relation (11.2) into account: fi (r)dV + Tij (r)nj dS = 0. V

S

Using Ostrogradsky’s theorem,1 we obtain: ∂Tij fi (r)dV + dV = 0 ∂xj V

and

V

fi (r) +

∂Tij dV = 0. ∂xj

V

Since this relation is valid whatever the volume V selected in the solid, we obtain fi +

∂Tij =0 ∂xj

which is the equilibrium relation we were seeking. 1. Ostrogradsky’s theorem states that for a vector ﬁeld A: ∂Aj divAdV = A · ndS or dV = Ak nk dS. ∂xj It can be generalized to the components of a tensor as: ∂Tij Tik nk dS = dV. ∂xj

(11.6)

Chapter 11 – The stress tensor

233

11.4. Symmetry of the stress tensor We now write that, for a solid at equilibrium, the total moment of the forces applied to it is zero. The component Mi of the moment M of a force F (M = r × F) with components Fk is (Sect. 10.6.2) Mi = δijk xj Fk where δijk is the Levi-Civita symbol, or permutation tensor (cf. Appendix 18A.2). Its value is 0 if two subscripts are equal, 1 if the permutation ijk is direct and −1 if it is inverse. The condition on the moment is expressed as: δijk xj fk dV + δijk xj Tkl nl dS = 0. Mi =

(11.7)

The second term can be written, using Ostrogradsky’s theorem:

∂Tkl ∂ (δijk xj Tkl )dV = δijk xj + Tkj dV δijk xj Tkl nl dS = ∂xl ∂xl where we used the fact that: ∂xj = δjl . ∂xl Further, using (11.6): ∂Tkl = −fk . ∂xl We obtain for this second term of (11.7): δijk xj Tkl nl dS = δijk (−xj fk + Tkj )dV and Equation (11.7) becomes: δijk xj fk dV + δijk (−xj fk + Tkj )dV = 0 or

δijk Tkj dV = 0

whatever the volume element dV . Hence δijk Tkj = 0. For i = 1, we obtain T32 − T23 = 0. In the same way, for i = 2 we obtain T13 = T31 and for i = 3 we have T21 = T12 . Thus we showed that Tij = Tji . The stress tensor is symmetric.

234

Symmetry and Physical Properties of Crystals

11.5. Examples of stress tensors In a material, the stress tensor Tij (r) results from the application of surface forces on the external surface Σ of the material, (Tn )Σ . Tij (r) is determined by solving Equations (11.4) with the boundary conditions on surface Σ given by the values of (Tn )Σ at all points of Σ. The solution of this kind of problems is dealt with in treatises on the mechanics of continuous media. In many cases, the solution is a non-uniform stress. It can nevertheless be considered as locally uniform by considering small volume elements, as we will do in the following paragraphs. In experiments designed to measure the elastic properties of materials, the shape of the objects and the applied force conﬁguration are usually designed so that the stress tensor is almost uniform (Sect. 13.1).

11.5.1. Uniaxial stress The stress tensor associated to a uniaxial stress is expressed, in a given frame (Ox1 x2 x3 ), by: ⎛ ⎞ T 0 0 ⎝ 0 0 0 ⎠. 0 0 0 Consider a small cube, with sides parallel to the coordinate axes, and with unit length (Fig. 11.6), and apply relation Tn = [T ]n to its faces. The faces normal to Ox2 and Ox3 are not submitted to any force. Vector n, associated to face ABCD, has the same direction as Ox1 , so that n = i and Tn = T i. If T is positive (as on Fig. 11.6), Tn is a tensile force2 and, if T is negative, Tn is a compressive force. Vector n associated to the opposite face of the cube, OFGH, is equal to −i, and Tn = −T i. We retrieve a tensile force if T is positive, and a compressive force if T is negative. x3 H D

G C

F

O i x1

A

x2

B

Figure 11.6: Uniaxial tensile stress applied on a small cube with unit sides 2. Tn is a force per unit area but here, for simplicity, we assume the surface areas to be equal to unity.

Chapter 11 – The stress tensor

235

11.5.2. Pure shear The stress tensor associated to a pure shear stress is expressed, in a given frame (Ox1 x2 x3 ), as: ⎛ ⎞ 0 T 0 ⎝ T 0 0 ⎠. 0 0 0 Consider, as above, a small cube with sides parallel to the coordinate axes, and with unit length. Figure 11.7 shows the forces acting on it if T is positive. x3

O

x2

x1

Figure 11.7: Pure shear stress acting on a small cube with unit sides If we rotate the coordinate system by 45◦ around Ox3 , the tensor, when expressed in this new set of axes, takes the form (Exercise 11.3): ⎛ ⎞ T 0 0 ⎝ 0 −T 0 ⎠ . 0 0 0 This is a bi-axial stress acting on the surfaces enclosing an angle of 45◦ wih the surfaces perpendicular to Ox1 and Ox2 (Fig. 11.8b).

11.5.3. Hydrostatic pressure Regardless of the orientation of the surface on which it acts, hydrostatic stress is normal to the surface and has the same value p. This stress is represented by tensor: ⎛ ⎞ −p 0 0 ⎝ 0 −p 0 ⎠ 0 0 −p which can be written as: Tij = −pδij , where δij is the Kronecker symbol. In this case, the three components dFi of the force dF acting on a surface element

236

Symmetry and Physical Properties of Crystals x2

x2 x’2

x’1

x1

x1

(a)

(b)

Figure 11.8: (a) Pure shear stress acting on the faces of a small cube with unit sides. (b) This stress is equivalent to a bi-axial stress involving tensile and compressive components, with the same norm, acting on faces at 45◦ to the initial ones. dS perpendicular to unit vector n, with direction cosines ni , are (Eq. 11.2): dFi = Tij nj dS = −p δij nj dS = −p ni dS and

dF = −p ndS

which means a force parallel to n and with value p dS whatever the orientation of n. The minus sign indicates that the pressure force points toward the inside of the volume element (compressive force).

11.6. Eﬀect of gravity Consider a bar in the shape of a rectangle parallelepiped with square crosssection and height h, resting in equilibrium on a plane surface (Fig. 11.9). This bar is submitted to no external stress on any of its faces, except for the one which rests on the surface (stress from the supporting surface). We choose a coordinate system (Ox1 x2 x3 ) parallel to the sides of the parallelepiped, with the axis Ox3 vertical and pointing downward, and the origin O in the plane of the upper face of the bar. The system of Equations (11.4) takes the form: ∂T1j =0 ∂xj ∂T2j =0 ∂xj ∂T3j + ρg = 0 ∂xj

(11.8a) (11.8b) (11.8c)

where ρ is the mass per unit volume of the material and g the acceleration of gravity.

Chapter 11 – The stress tensor

237 O

x1

x2

h

x3

Figure 11.9: Bar in the shape of a rectangle parallelepiped with square cross-section, with height h, resting in equilibrium on a plane surface The faces perpendicular to Ox1 and Ox2 are submitted to no stress, so that Tj2 = Tj1 = 0 on the faces. In a ﬁrst approximation, we may therefore consider that, in a cross section of the bar at x3 = const, the stress is uniform, so that Tj2 = Tj1 = 0 and Tj3 = const over the whole surface. We deduce that:

∂Tj2 ∂Tj2 ∂Tj1 ∂Tj1 = = = =0 ∂x2 ∂x1 ∂x1 ∂x2

and in particular ∂T32 ∂T31 = = 0. ∂x2 ∂x1 Equation (11.8c) then reduces to: ∂T33 + ρg = 0. ∂x3 The solution of this equation is: T33 = −ρgx3 + C(x3 ). C is a constant which depends neither on x1 nor on x2 since the stress is supposed to be uniform at constant x3 . Face x3 = 0 is submitted to no stress, hence T33 (x3 = 0) = 0. We deduce that C(x3 ) = 0 and that T33 = −ρgx3 . On the lower face of the bar (x3 = h), T33 = −ρgh. The force acting on this face of the bar, with area S, is then equal to −ρghS, i.e. to −P if P is the weight of the bar. The surface on which it rests exerts upon the bar a force equal and opposite to its weight, as expected.

238

Symmetry and Physical Properties of Crystals

In metallurgy, test specimens have height around 100 mm. The stress due to gravity therefore varies from zero to the maximum value ρgh which, in the case of a steel specimen for example (ρ = 7.8 kg dm−3 ) is equal to (7.8 × 103 ) × 9.81 × 0.1 = 7.7 × 103 Pa. This stress is therefore completely negligible with respect to the stresses, of the order of a MPa, applied to the specimens in the elastic range. Gravity can thus be neglected.

11.7. Exercises Exercise 11.1 Consider a uniaxial stress T acting on a surface perpendicular to the vector n, with direction cosines n1 , n2 , n3 in an orthonormal axis system (Ox1 x2 x3 ). Determine the components of the stress tensor in the axis system (Ox1 x2 x3 ). First express the tensor in a system of axes where one of the axes, say Ox1 , is parallel to n, and then perform the axis change. Exercise 11.2 Consider a stress tensor which, in a given orthonormal axis system (Ox1 x2 x3 ), takes the form: ⎛ ⎞ 0 0 0 ⎝ 0 0 0 ⎠. 0 0 T 1.

Calculate the moduli Tν and τ of the normal and shear stresses respectively, to which a surface perpendicular to the unit vector n with direction cosines n1 , n2 , n3 is submitted.

2.

For what directions of vector n is the shear stress maximum?

Exercise 11.3 Consider a pure shear tensor represented in an orthonormal axis system (Ox1 x2 x3 ) by: ⎛ ⎞ 0 T 0 ⎝ T 0 0 ⎠. 0 0 0 Give the form of this tensor in an axis system deduced from (Ox1 x2 x3 ) by a 45◦ rotation around Ox3 . Exercise 11.4 The stress tensor [T ] at a point M in a material is given, in an orthonormal axis system (Ox1 x2 x3 ), by: ⎛ ⎞ 0.7 3.6 0 ⎝ 3.6 2.8 0 ⎠ 107 N m−2 . 0 0 7.6

Chapter 11 – The stress tensor

239

1.

Determine the principal stresses and their directions.

2.

Retrieve these results using the Mohr circle method.

3.

Calculate the stress T acting √ on a small surface, centered at M, whose normal has direction cosines ( 3/2, 1/2, 0). Find the normal stress and shear stress components.

240

Symmetry and Physical Properties of Crystals

References [1] D. Calecki, Physique des milieux continus, vol. 1, Mécanique et thermodynamique (Hermann, Paris, 2007) [2] L.D. Landau and E.M. Lifshitz, Course of Theoretical Physics, vol. 7, Theory of Elasticity, 3rd edn. (Elsevier, Oxford, 1986)

Chapter 12

Deformation of a solid. The strain tensor This chapter introduces the displacement gradient tensor, or distortion tensor, which describes the most general distortion of a crystal. This ﬁeld tensor of rank 2 is shown to decompose into the strain tensor, which is symmetric, and an antisymmetric tensor associated to a rotation. The last section is devoted to the thermal expansion of crystals.

12.1. Distortion tensor (displacement gradient tensor) 12.1.1. Deﬁnition We consider a material submitted to a deformation. This deformation displaces point P, deﬁned by its position vector OP = r, to point P such that PP = u(r) (Fig. 12.1). Vector u(r) is the displacement vector at point P. It is not uniform, because if it were, the whole material would simply be translated and it would not be deformed. A neighboring point Q such that PQ = Δr displaces to Q such that QQ = u(r + Δr). x3

Q’

r’ P’

u(r + r)

u(r) P

r

Q

O

x2

x1

Figure 12.1: Transformation of vector PQ= Δr into vector P Q = Δr after deformation

© Springer Science+Business Media Dordrecht 2014 C. Malgrange et al., Symmetry and Physical Properties of Crystals, DOI 10.1007/978-94-017-8993-6_12

241

242

Symmetry and Physical Properties of Crystals

Vector PQ becomes, after transformation, vector P Q = Δr such that: P Q = P P + PQ + QQ Δr = Δr + u(r + Δr) − u(r)

so that

Δr = Δr + Δu

or

(12.1)

if we note Δu = u(r + Δr) − u(r). We can replace u(r + Δr) by its expansion to ﬁrst order, and thus obtain for the three components of Δu: Δui =

∂ui Δxj . ∂xj

(12.2)

∂ui = eij , ∂xj

Setting

Δui = eij Δxj .

we obtain:

(12.3)

Coeﬃcients eij connect the components of a vector Δr to the components of vector Δu. They are therefore the components of a tensor (see Sect. 9.4.2) called the displacement gradient tensor, or distortion tensor, and we can write: Δu = [e]Δr. Thus

Δr = Δr + [e]Δr = ([E] + [e])Δr

or

Δxi

(12.4) (12.5)

= Δxi + eij Δxj = (δij + eij )Δxj

where [E] is the unit tensor. If components eij do not depend on the position of the point, the distortion is uniform, and there are no additional terms in the expansion (12.2). Relations (12.4) and (12.5) are then valid even if points P and Q are not near each other, and the linear relation between Δr and Δr shows that a line remains a line and a plane remains a plane after distortion. If the eij vary from point to point, the distortion is no more uniform, but Equations (12.4) and (12.5) remain valid locally, which implies small Δr. We can thus consider, as is done in this chapter, that the distortions are uniform: if they are not, the properties obtained are valid locally. Further, we will only consider, in what follows, very small displacement gradients (distortions), i.e. eij 1.

Chapter 12 – Deformation of a solid. The strain tensor

243

12.1.2. Physical meaning of components eij We will simplify the interpretation of components eij by considering a twodimensional system, in which we choose an orthonormal axis system (Ox1 x2 ). Equations (12.3) now become the following detailed equations: Δu1 = e11 Δx1 + e12 Δx2 ,

(12.6)

Δu2 = e21 Δx1 + e22 Δx2 .

(12.7)

Consider a rectangle whose sides PQ and PS, respectively parallel to Ox1 and Ox2 , have components (Δx1 , 0) and (0, Δx2 ) respectively. Vectors PQ and PS become, after deformation, P Q and P S respectively. Consider for a start vector PQ, which turned into P Q , and apply relations (12.6) and (12.7): Δu1 = e11 Δx1 , Δu2 = e21 Δx1 . PQ has rotated by angle θ, and its length has changed. As we immediately see on Figure 12.2, tan θ = Δu2 /(Δx1 + Δu1 ). Since we assume that eij 1, Δu1 and Δu2 are much smaller than Δx1 and tan θ ∼ = Δu2 /Δx1 = e21 , and tan θ ∼ θ. We can write: = θ = e21 . Thus e21 is the angle by which PQ, parallel to Ox1 , has rotated. It is counted as positive in the sense from Ox1 to Ox2 (direct sense). The same argument applied to PS shows that e12 is the angle θ by which PS, parallel to Ox2 , has turned, counting it as positive from Ox2 to Ox1 (clockwise).1 x2

R’ S’ ’

S

R P’

x2

x1

u1

Q

P O

Q’ u2

x1

x1

Figure 12.2: Distortion of rectangle PQRS, which becomes P Q R S . The lengths Δu 1 and Δu 2 are hugely magniﬁed in order to make angle θ visible.

1. It is obvious that, to keep Figure 11.2 and the following ones clear, it is necessary to show lengths Δu1 and Δu2 much larger than in reality. Therefore, they do not satisfy the condition eij 1, and angles θ and θ are also too large.

244

Symmetry and Physical Properties of Crystals

We now calculate the variation in length Δx1 of PQ, which became P Q : we have P Q − PQ = P Q − Δx1 . We see on Figure 12.2 that Δx1 + Δu1 = P Q cos θ ∼ = P Q since θ 1. Thus P Q ∼ = PQ + Δu1 , and we obtain Δu1 P Q − PQ = e11 . = PQ Δx1 The relative elongation of PQ is thus equal to e11 . The same argument applied to PS shows that e22 is the relative elongation of PS, parallel to Ox2 . These results are easily generalized to three dimensions. We can thus state that: each diagonal term2 eii in the distortion tensor represents the relative elongation of a segment parallel to axis Oxi , the components eij , where i = j, describe the rotation of these segments.

12.2. Decomposition of the distortion tensor into a rotation and a strain 12.2.1. Introduction using a simple example Consider the very simple distortion tensor ⎛ 0 −α ⎝α 0 0 0

[T ] represented by matrix ⎞ 0 0⎠ . 0

This distortion does not aﬀect a vector parallel to Ox3 , and we can therefore focus on the distortion in plane (Ox1 ,Ox2 ) and investigate what a small square PQRS becomes after distortion (Fig. 12.3). The diagonal terms being zero, the segments parallel to Ox1 and Ox2 retain their lengths. Segment PQ undergoes a rotation by α in the direct sense and segment PS a rotation −α in the clockwise direction, i.e. a rotation by α in the direct sense. Thus the square has been transformed into an identical square, rotated by angle α in the direct sense. This shows that there are distortions which do not deform the solid, but just rotate it.

2. Here, Einstein’s convention does not apply to notation eii , i.e. no sum is implied.

Chapter 12 – Deformation of a solid. The strain tensor

245

R’ x2

S’

S

R

Q’

P’

P

Q

O

x1

Figure 12.3: Transformation of square PQRS when submitted to a special distortion involving a simple rotation

12.2.2. Expressing the distortion associated to small rotations Consider a small rotation by angle dα around an axis with unit vector n going through point O. Let M be the transform of point M in this rotation (Fig. 12.4). OM = OM + MM . The plane perpendicular to the rotation axis, going through M, intersects this axis at H.

H

d

M’ M

n O

Figure 12.4: Transformation of vector OM into vector OM through a small rotation, by angle d α, around an axis with unit vector n going through point O Since we assume angle dα to be very small, arc MM and its tangent at M are very close to each other. MM is perpendicular to n and also to HM since the rotation angle dα is small. MM , being perpendicular to plane (OH, HM), is thus perpendicular to OM and to n, hence parallel to vector n × OM. Its length MM is MM = HM dα = OM sin θ dα

246

Symmetry and Physical Properties of Crystals

where θ is the angle between OM and n. We thus obtain MM = (n × OM) dα OM = OM + (n × OM) dα.

and

(12.8)

If we denote as ni the components of n and xi the components of OM in any given orthonormal axis system (Ox1 x2 x3 ), the vector n × OM has for components, in this axis system ⎧ ⎨ n 2 x3 − n 3 x2 n x − n 1 x3 ⎩ 3 1 n 1 x2 − n 2 x1 and Equation (12.8) can be written as OM = ([E] + [Ω])OM where [Ω] is a tensor (since it relates vector OM − OM to vector OM) which, in the orthonormal basis chosen, is expressed as ⎞ ⎛ n2 0 −n3 0 −n1 ⎠ [Ω] = ⎝ n3 −n2 n1 0 and [E] is the unit tensor. We deduce that any vector r transforms, under rotation by a small angle dα around n, into vector r such that r = ([E] + [Ω])r

(12.9)

where [Ω] is an antisymmetric tensor. We note that the special case we discussed in Section 12.2.1 satisﬁes this result. Since this relation is linear, it applies to any vector Δr, irrespective of whether its origin is on the rotation axis. Relation (12.9) then becomes: Δr = ([E] + [Ω])Δr or

Δu = Δr − Δr = [Ω]Δr.

[Ω], an antisymmetric tensor, is associated to the rotation vector ndα. We thus ﬁnd a second example of an axial vector, the rotation vector ndα being equivalent to the antisymmetric second-rank tensor [Ω]dα (see Sect. 10.6.2).

12.2.3. Strain tensor A general distortion tensor can be decomposed into the sum of a symmetric tensor [S] and an antisymmetric tensor [A] (Sect. 10.1.1), which we will denote here as [Ω], such that: Sij =

eij + eji 2

Ωij =

eij − eji , 2

Chapter 12 – Deformation of a solid. The strain tensor so that

∂uj 1 ∂ui + 2 ∂xj ∂xi

∂uj 1 ∂ui . − Ωij = 2 ∂xj ∂xi Sij =

247

(12.10) (12.11)

Relation (12.5) becomes Δr = ([E] + [e])Δr = ([E] + [S] + [Ω])Δr. The distortions we consider here are always small, hence eij 1, and we can write: ([E] + [S] + [Ω]) ∼ = ([E] + [S])([E] + [Ω]), and

Δr = ([E] + [S])([E] + [Ω])Δr.

The transformation of vector Δr into Δr is the product of a rotation ([E]+[Ω]) and a deformation ([E] + [S]).3 [S] is the symmetric part of the distortion tensor: it is called the strain tensor. [Ω], its antisymmetric part, is called the rotation tensor. Generally, interest focuses only on the change in shape of the object, hence on the strain tensor [S], a symmetric tensor. The diagonal terms in [S] are equal to those of [e], and they thus represent relative elongations (see Sect. 12.1.2). Thus S11 represents the relative elongation of a segment parallel to axis Ox1 , S22 that of a segment parallel to Ox2 and S33 that of a segment parallel to Ox3 . The strain tensor is a ﬁeld tensor. It usually results from another ﬁeld tensor being applied to the crystal, for example a stress, deﬁned in Chapter 11, an electric ﬁeld if the crystal is piezoelectric (Chap. 15), or a variation in temperature as we will see in Section 12.6.

12.3. Elongation in a given direction There is often interest in the relative elongation, in a given direction parallel to unit vector s, of a material submitted, in the vicinity of point P, to a given strain tensor [S]. If [S] is uniform, Δ/|s represents the relative elongation of a bar parallel to s. The tensor is given through its components Sij in a given orthonormal axis system (Ox1 x2 x3 ). Let (Ox1 x2 x3 ) be a new orthonormal axis system such that Ox1 is parallel to s. We saw in last section that the relative elongation in direction Ox1 is given by S11 . Thus Δ = S11 = a1i a1j Sij , s 3. The order of the operations is irrelevant: since Ωij 1 and Sij 1, ([E] + [S])([E] + [Ω]) ∼ = ([E] + [Ω])([E] + [S]).

248

Symmetry and Physical Properties of Crystals

where {aij } is the transformation matrix leading from axis system (Ox1 x2 x3 ) to axis system (Ox1 x2 x3 ). The basis vector e1 of the new system is none other than s, hence a1i = si . We obtain Δ = si sj Sij (12.12) s or, in matrix form, ⎛ Δ = s1 s2 s3 ⎝ s

⎞⎛ Sij

⎞ s1 ⎠ ⎝ s2 ⎠ . s3

This relative elongation is equal to the reciprocal of the square of the radius vector of the quadric associated to tensor [S] (Sect. 10.3.2).

12.4. Volume expansion (volumetric strain) When described in the axis system (Ox1 x2 x3 ) of its principal axes, a strain tensor [S], with components Sij , is diagonal. Consider a small rectangle parallelepiped with sides parallel to Ox1 , Ox2 and Ox3 and with lengths respectively Δx1 , Δx2 , Δx3 (Fig. 12.5). x3 x2(1+S22) x1(1+S11) x1 O

x2

x3

x3(1+S33) x2

x1

Figure 12.5: A rectangle parallelepiped with sides parallel to principal axes Ox 1 , Ox 2 and Ox 3 , with lengths respectively Δx 1 , Δx 2 , Δx 3 , shown before and after deformation This rectangle parallelepiped, with volume ΔV equal to Δx1 Δx2 Δx3 , becomes, under this deformation, another rectangle parallelepiped since only the diagonal terms of the tensor are non-zero. Its sides have lengths respectively Δx1 (1 + S11 ), Δx2 (1 + S22 ) and Δx3 (1 + S33 ). The volume ΔV of the deformed parallelepiped is: ΔV = ΔV (1 + S11 )(1 + S22 )(1 + S33 ) ≈ ΔV (1 + S11 + S22 + S33 ).

Chapter 12 – Deformation of a solid. The strain tensor

249

The relative variation in volume is: ΔV − ΔV = S11 + S22 + S33 , ΔV equal to the trace of the matrix representing tensor [S] in the coordinate system of its principal axes. We saw (Sect. 10.1.3) that the trace of a tensor is independent of the coordinate system in which it is expressed. Therefore the relative variation in volume (volume expansion, or volumetric strain) is equal to the trace of the strain tensor whatever the coordinate system in which the tensor is expressed.

12.5. Special cases of strain 12.5.1. Simple elongation The strain tensor associated to simple elongation, expressed in a given axis system (Ox1 x2 x3 ), has a single non-zero term, located on the diagonal; for example: ⎛ ⎞ 0 0 0 ⎝ 0 0 0 ⎠. 0 0 S A small rectangle parallelepiped with sides parallel to the axes and with lengths respectively Δx1 , Δx2 , Δx3 remains a rectangle parallelepiped, in which only the side parallel to Ox3 has suﬀered a relative elongation equal to S.

12.5.2. Pure shear strain The associated strain tensor is expressed, in a given coordinate system (Ox1 x2 x3 ), as: ⎛ ⎞ 0 S 0 ⎝ S 0 0 ⎠. 0 0 0 It is easy to show (Exercise 12.2) that, in the coordinate system (Ox1 x2 x3 ) rotated by 45◦ around axis Ox3 , this tensor takes on the form: ⎛ ⎞ S 0 0 ⎝ 0 −S 0 ⎠ 0 0 0 which corresponds to an expansion along Ox1 and a contraction along Ox2 . A small square PQRT, with sides parallel to Ox1 and Ox2 respectively, becomes after deformation a lozenge (Fig. 12.6). The length of the sides of the lozenge is equal to that of the square since, in the initial coordinate system, S11 = S22 = 0.

250

Symmetry and Physical Properties of Crystals x2

T

R’

T’

R

S

P

S

Q’ Q

O

x1

Figure 12.6: Pure shear of the small square PQRT, with sides parallel to Ox 1 and Ox 2 , which becomes the lozenge PQ R T

12.5.3. Simple shear strain The distortion tensor [e] in simple shear is expressed in a given frame (Ox1 x2 x3 ) as: ⎛ ⎞ 0 γ 0 ⎝ 0 0 0 ⎠. 0 0 0 A small square PQRS with sides parallel to Ox1 and Ox2 becomes, after this distortion, a lozenge PQR S because the tensor has no diagonal terms (Fig. 12.7a). The side parallel to Ox2 rotates by −γ (see Sect. 12.2.1). Because the tensor is not symmetric, we decompose it into a strain and a rotation: ⎛ ⎞ ⎛ ⎞ 0 γ/2 0 0 γ/2 0 [S] = ⎝ γ/2 0 0 ⎠ and [Ω] = ⎝ −γ/2 0 0 ⎠ . 0 0 0 0 0 0 Simple shear thus consists in the combination of a rotation by angle −γ/2 around Ox3 and pure shear (Fig. 12.7b).

12.6. Thermal expansion Suppose we submit a bar of an isotropic material, with length 0 at temperature T0 , to a temperature change ΔT . Its length becomes such that: = 0 (1 + αΔT ) where α is the linear thermal expansion coeﬃcient of the material. In a general way, an isotropic solid submitted to a uniform rise in temperature expands while retaining its shape, and vector Δr in the material becomes, after a change in temperature ΔT , a vector Δr parallel to Δr and such that: Δr = Δr(1 + αΔT ) = Δr + Δu

Chapter 12 – Deformation of a solid. The strain tensor

251

x2 S S’’

R R’’

S S’ S’’ x3

– f

P

R R’’ R’

–– f 2

Q

Q Q’

P

(a)

x1

(b)

Figure 12.7: (a) Simple shear of the small square PQRS, which becomes lozenge PQR S . (b) This transformation can be decomposed into two successive transformations: rotation by −γ/2 (the square PQRS becomes square PQ R S ), and then a deformation of PQ R S analogous to that of Figure 12.6. Δu = αΔT Δr.

with

If the solid is not isotropic, the vector Δu is, in general, no more parallel to Δr and its expression at a function of Δr is given by a strain tensor [S] proportional to the change in temperature ΔT : Δu = [S]Δr = [α]ΔrΔT or and

Δui = αij Δxj ΔT, Sij = αij ΔT.

(12.13)

Tensor [α] thus deﬁned is the thermal expansion tensor. This second-rank tensor is symmetric and represents a physical property of the material. It relates an external applied constraint (the change in temperature) to the eﬀect it induces (strain). It is a material tensor, which must be invariant with respect to the crystal’s symmetry elements. The number of independent coeﬃcients of symmetric rank-2 tensors was determined (Sect. 10.5) for the various point groups. This number depends only on the crystal system because it is found to be identical for all the point groups of a given crystal system. We thus obtain for the various crystal systems the following results: Triclinic system: 6 independent coeﬃcients. Monoclinic system: one principal axis of the tensor is parallel to the 2-fold axis (groups 2 and 2/m) or perpendicular to the mirror (group m). There are four independent coeﬃcients. The ellipsoid representing the tensor has one of its axes parallel to the 2-fold axis or perpendicular to the mirror. Orthorhombic system: the principal axes are parallel to the 2-fold axes or perpendicular to the mirrors. They are the axes of the ellipsoid representing the tensor. There are three independent coeﬃcients.

252

Symmetry and Physical Properties of Crystals

Tetragonal, rhombohedral and hexagonal systems: the ellipsoid representing the tensor is an ellipsoid of revolution around the axis with order larger than 2. There are two independent coeﬃcients. Cubic system: the representation ellipsoid is a sphere. The crystal behaves with respect to thermal expansion as an isotropic material. There is only one coeﬃcient. We note that the strain induced by a change in temperature is uniform if the temperature is uniform. The coeﬃcients αij are in general all positive. Nevertheless there are a few cases where one of the coeﬃcients is negative (calcite or beryl for example). In these special cases, there are directions in which the expansion coeﬃcient is zero. Consider for example calcite, with point group ¯3m, for which the thermal expansion tensor [α] is expressed as: ⎛ ⎞ −5 0 0 ⎝ 0 −5 0 ⎠ 10−6 ◦ C−1 0 0 27 when expressed in an axis system where Ox3 is parallel to the 3-fold axis.4 The relative elongation Δ/|s , in a given direction with unit vector s, is given by Equation (12.12): Δ = si Sij sj = si sj αij ΔT. s If ΔT = 1◦ C, we obtain for calcite: Δ = [−5(s21 + s22 ) + 27s23 ] 10−6 s

which, expressed in spherical coordinates, becomes: Δ = [−5sin2 θ + 27cos2 θ] 10−6 . s The surface representing this relative elongation is obtained by giving any segment parallel to s drawn from a given point O the length Δ/|s . Here it is a surface of revolution around Ox3 . Figure 12.8a shows a section of this surface by a plane going through this axis of revolution. We see that

Δ =0 s

if

tan2 θ =

27 5

thus for all direction at angle θ = θ0 = 66.7◦ (or its supplement θ = 113.3◦ ) to axis Ox3 . 4. We recall that a ¯ 3-fold axis is equivalent to a 3-fold axis and a center of symmetry.

Chapter 12 – Deformation of a solid. The strain tensor x3

253

x3

+ o

_

o

_

+

(a)

(b)

Figure 12.8: Thermal expansion of a crystal of calcite. The 3-fold axis, chosen for the axis Ox 3 , is an axis of revolution and the ﬁgures represent any plane (Oρ, Ox 3 ) going through Ox 3 . (a) Relative elongation for all directions of a plane going through axis Ox 3 . (b) Transformation of a sphere with unit radius, which becomes an ellipsoid of revolution around Ox 3 . The deformations are hugely exaggerated in order to be visible. We saw (Eq. (10.6)) that, for a given tensor with components Tij , the quantity Tij si sj is equal to 1/r 2 where r is the length of the radius vector of the representation quadric for the tensor, deﬁned by Tij si sj = 1. This remark makes it possible to retrieve the above result, viz. the fact that in the directions of the cone asymptotic to the hyperboloids −5(x21 + x22 ) + 27x23 = ±1, the relative elongation is zero since r → ∞. For those directions that enclose with Ox3 an angle smaller than the half-angle of the cone, the representation of the quadric is a two-sheet hyperboloid with equation αij xi xj = 1 and the relative elongation is then equal to 1/r 2 . For directions that are outside this cone, the quadric is a one-sheet hyperboloid with equation αij xi xj = −1 and the elongation is equal to −1/r 2 . Figure 12.8b shows that a sphere with unit radius becomes, through thermal expansion, an ellipsoid with an expansion in the direction Ox3 and a contraction in all directions of plane (Ox1 , Ox2 ). We note that, in direction θ0 , although the radius vector does not expand, it nevertheless undergoes a transformation which is then only a rotation (Exercise 12.5). Any change in temperature of a solid leads to a relative variation ΔV /V of its volume V . As we saw in Section 12.4, ΔV /V is the trace of the strain tensor: ΔV = Sii = αii ΔT = (α11 + α22 + α33 )ΔT V The bulk thermal expansion is αii . If the material is isotropic, with linear expansion coeﬃcient α, we obtain ΔV /V = 3αΔT , as expected.

254

Symmetry and Physical Properties of Crystals

When it is expressed in the coordinate system of its principal axes, tensor [α] is diagonal, and its diagonal terms α11 , α22 , α33 are called the principal expansion coeﬃcients. For simplicity, they are noted α1 , α2 , α3 respectively. A few examples of the numerical values of these coeﬃcients are given in Table 12.1, in units of 10−6 ◦ C−1 . Table 12.1: Principal expansion coeﬃcients for some crystals, in units of 10−6 ◦ C−1 α1

α2

α3

10.8

10.8

64.5

around − 210◦ C

−2

−2

55

Rhombohedral

around 25◦ C

13.4

13.4

7.97

Calcite

Rhombohedral

40◦ C

−5

−5

27

Copper

Cubic

around 25◦ C

16

16

16

Silicon

Cubic

around 25◦ C

2.35

2.35

2.35

Crystal

Crystal system

Zinc

Quartz

Hexagonal

Temperature range 30 to

118◦ C

around

12.7. Exercises Exercise 12.1 A material is distorted in such a way that the components of the displacement u(P) at a point P with coordinates (x1 , x2 , x3 ) in an orthonormal axis system are: u1 = 2 × 10−5 x1 − 10−5 x2 u2 = 2 × 10−5 x1 − 2 × 10−5 x2 u3 = 0 1.

Determine the components eij = ∂ui /∂xj of the distortion tensor [e]. Decompose tensor [e] into the strain tensor and the rotation tensor.

2.

Determine the relative elongation of a segment in a direction parallel to the vector with components (1, 1, 1).

Exercise 12.2 A uniform strain tensor is represented in an orthonormal axis system (Ox1 x2 x3 ) by the matrix: ⎛ ⎞ 0 S 0 ⎝ S 0 0 ⎠. 0 0 0

Chapter 12 – Deformation of a solid. The strain tensor

255

1.

How does this strain transform a square with sides being parallel to Ox1 and Ox2 respectively and with unit length?

2.

Determine the principal values and the principal axes of this tensor.

Exercise 12.3 Consider a homogeneous bar with the shape of an elongated rectangle parallelepiped (see ﬁgure below). Choose an axis system such that Ox1 is parallel to the long side of the bar, Ox2 and Ox3 being parallel to the two other sides. This bar undergoes a uniform strain, the principal axes of which are Ox1 , Ox2 and Ox3 , and the principal values S11 = η, S22 = −0.3η, S33 = −0.3η with η = 10−4 . A line with length L, drawn on the bar in plane (Ox1 , Ox2 ) in the undeformed state, encloses angle α with Ox1 before deformation. x2 L

x1

1.

Calculate the relative elongation of the line.

2.

After deformation, the line encloses with Ox1 the angle α = α + ε. Calculate the small angle ε.

Exercise 12.4 A small distortion of a crystal is deﬁned ⎛ 4 2 eij = ⎝ −4 1 6 0

by the following tensor: ⎞ −2 0 ⎠ 10−6 . 3

Determine the strain tensor Sij and the rotation tensor Ωij . Find the principal axes of tensor [S], the rotation axis and the angle of rotation Δα corresponding to tensor [Ω]. Exercise 12.5 Graphite is hexagonal, with point group 6mm. In order to determine the coeﬃcients of the thermal expansion tensor, the lattice parameters of a graphite crystal were measured at 20◦ C and at 100◦ C. At 20◦ C, the values are: a20 = 2.4560 Å, c20 = 6.6960 Å. At 100◦ C, they are: a100 = 2.4557 Å, c100 = 6.7110 Å.

256

Symmetry and Physical Properties of Crystals

1.

Calculate, in this temperature range, the average thermal expansion tensor5 of graphite. Indicate what axis system it is expressed in.

2.

Calculate the average thermal expansion coeﬃcient in a general direction at angle θ to the 6-fold axis. Show that there are directions in which the elongation is zero, and that these directions form a cone; determine its apical angle θ0 . Give a graphical interpretation of this result using the representation quadric of this tensor.

3.

Show that this special direction undergoes, in a temperature variation, a small rotation; calculate it.

Exercise 12.6 Consider a crystal of rutile TiO2 , with tetragonal symmetry and lattice parameters a = b = 4.5933 Å and c = 2.9592 Å at 0◦ C. When it is heated from 0◦ C to 100◦ C, the angle between planes (100) and (101) decreases by 0.095 mrad. Given that the average bulk expansion between 0◦ C and 100◦ C is 23.4 × 10−6 ◦ C−1 , calculate the two principal expansion coeﬃcients of this crystal. Exercise 12.7 Barium titanate BaTiO3 undergoes several phase changes (or phase transitions) at various temperatures: above 120◦ C, BaTiO3 is cubic. At 120◦ C it becomes tetragonal, and remains so down to 0◦ C. At 0◦ C, BaTiO3 becomes orthorhombic and remains so down to −100◦ C, when it becomes rhombohedral. The point symmetry group and the lattice parameters of the various phases are given in the table below. System P. G. T

Cubic m¯3m

Tetragonal Orthorhombic Rhombohedral 4mm mm2 3m ◦ ◦ ◦ 120 C 0 C − 100 C 120◦ C 120◦ C 0◦ C – 100◦ C a = 4.010 Å a = b = 4.002 Å bm = cm = 4.012 Å a = 3.996 Å c = 4.021 Å am = 3.988 Å α = 89.86◦ ◦ ◦ 0 C α = 90.20 a = b = 3.991 Å – 100◦ C c = 4.034 Å bm = cm = 4.012 Å am = 3.978 Å α = 90.40◦

5. The lattice parameters do not vary linearly with temperature. The data given only allow calculating the average thermal expansion coeﬃcients.

Chapter 12 – Deformation of a solid. The strain tensor

257

In the cubic ↔ tetragonal transformation, the directions of the basis vectors remain unchanged. In the tetragonal ↔ orthorhombic transformation, the direction of a is unchanged. The rectangular face (b, c) becomes a lozenge with side bm = cm = a and with angle α = 90◦ , deﬁning a monoclinic pseudo-unit cell. The orthorhombic unit cell is a unit cell with twice the volume of this one. The basis vector ao is parallel to the vector ac of the cubic unit cell. The vectors bo and co are respectively parallel to the diagonals of the lozenge faces of the monoclinic pseudo-unit cell. The 3-fold axis of the rhombohedral phase coincides with one of the 3-fold axes of the cubic phase. 1.

Calculate the components of the average6 thermal expansion tensor of BaTiO3 in the tetragonal phase. Deduce the expansion coeﬃcient for a general direction. Does it vanish for some directions? Which ones?

2.

Calculate the norms of the basis vectors of the orthorhombic unit cell at 0◦ C and at −100◦ C. Determine the thermal expansion tensor in this phase (express it in the orthonormal axis system parallel to the basis vectors of the orthorhombic unit cell).

3.

Calculate the components of the strain tensor corresponding to the transition from the cubic cell (at 120◦ C) to: (a) the tetragonal unit cell at 120◦ C, (b) the orthorhombic unit cell at 0◦ C, (c) the rhombohedral unit cell at −100◦ C. Indicate, in each case, the axis system in which the tensors are expressed.

6. See the note for Exercise 12.5.

Chapter 13

Elasticity The stiﬀness and compliance tensors, which relate the stress tensor to the resulting strain tensor, are symmetric tensors of rank 4. This chapter shows how the intrinsic symmetry of the strain and stress tensors reduces the number of independent components of the compliance and stiﬀness tensors, and then how the symmetry of the crystal, described by its point group, can further reduce this number. A short notation, called Voigt’s notation, is often used for these tensors. It represents the stress and the strain tensors through 6-component vectors, and the compliance and stiﬀness tensors by symmetric 6 × 6 matrices which are inverse to each other.

13.1. Introduction In this chapter, we investigate the deformation of a crystalline material under the inﬂuence of a given stress. We ﬁrst need to know the stress acting at any point in the material. We saw (Sect. 11.5) that the stress tensor Tij (r) in a material results from the application of surface forces on the external surface Σ of the material. For measurements to have an easy interpretation, the shape of the material and the conﬁguration of the external forces to be applied are designed so that the stress tensor is practically uniform. The most usual experiments consist in measuring the strain resulting from a uniaxial stress. The typical specimen shape for this use is shown on Figure 13.1. 0 S

F

F

5 cm

(a)

(b)

Figure 13.1: (a) Photograph of a tensile test specimen; (b) schematic diagram of a traction experiment. The uniaxial stress T in the central part, with cross section S, is T =F /S.

© Springer Science+Business Media Dordrecht 2014 C. Malgrange et al., Symmetry and Physical Properties of Crystals, DOI 10.1007/978-94-017-8993-6_13

259

260

Symmetry and Physical Properties of Crystals

It consists of a long central cylindrical part with constant cross section, and of two ends with a cross section larger than the central part. The transition between the central part and the ends occurs progressively. The ends of these specimens are secured to the grips. One of them is ﬁxed and the other one submitted to a traction force F. The stress tensor in the central part, with cross section S, can then be shown to be practically uniform. The stress is uniaxial and its value is T = F/S. As a result, the length of the constant cross section part of the specimen increases from the zero-stress value 0 to = 0 + Δ. The elongation Δ depends on the value of the stress. The deformation curves are usually represented by plotting the relative elongation Δ/ horizontally and the stress vertically. The general trend is given on Figure 13.2, where we note that the initial part is a straight line. T Elastic range

Plastic range Fracture

0

Figure 13.2: Deformation curve of a material submitted to a tensile stress. The linear part of this curve is the elastic deformation range. This diagram (T , Δ/) shows several stages in the deformation process: 1. The elastic deformation range For small values of T , the material has a linear behavior. The elongation is proportional to the applied stress: 1 Δ = T. E This is Hooke’s law, and E is Young’s modulus of the material, assumed to be isotropic. In this stress range, the material recovers its initial dimensions when the stress is removed: the transformation is reversible. Young’s modulus is a measure of the mechanical property called stiﬀness or rigidity. The larger Young’s modulus, the more rigid is a material, and therefore the smaller is its elastic deformation for a given value of the stress. Actually, Young’s modulus is not suﬃcient to completely characterize the deformation of the bar, because the cross section of the bar also changes. If the cross section is circular, it remains circular in an isotropic material, and

Chapter 13 – Elasticity

261

its diameter d undergoes a relative contraction, noted Δd/d (with Δd < 0), also proportional to the stress. The absolute value of the ratio between this relative contraction and the relative elongation of the bar is called Poisson’s ratio, noted ν: ν=−

Δd/ d Δ/

so that we can write:

ν Δd = − T. d E We note that, in this range, the volume of the material changes because the elongation is generally not totally compensated by the decrease in cross section. This volume change is noted as: Δ 2Δd 1 − 2ν ΔV = + = T. V d E The order of magnitude of Young’s modulus E for metals is some 1010 N m−2 , and Poisson’s coeﬃcient ν is generally close to 0.3 for usual metals. 2. The plastic range Beyond the elastic range, the strain-stress curve shows a plateau which can be more or less extended depending on the material. This is the plastic deformation range, where deformation occurs at almost constant volume. In this range, which involves the displacement and multiplication of defects called dislocation lines,1 the material retains some permanent deformation when the stress is released. The deformation in this range is thus not reversible. The boundary between the two ranges we just deﬁned is called the elastic limit, or yield strength. It is related to the defects in the solid, and is therefore an extrinsic property of the material, variable from one specimen to another. The order of magnitude of this elastic limit for metals is some 107 to some 108 N m−2 . In practice, this limit is often diﬃcult to pinpoint because the transition from the elastic to the plastic range is continuous. 3. The breaking range In this range, the deformation is localized: the cylinder necks at a point and breaks. This type of diagram assumes that the stress and strain are simultaneous, i.e. that the deformation sets in as soon as the stress is applied. This is the case for metals and many solids. These materials are called elastic materials. Their behavior in a deformation experiment is not inﬂuenced by the stress rate, and 1. A brief introduction to dislocations is given in the complement to this chapter.

262

Symmetry and Physical Properties of Crystals

it is well described by Hooke’s law, independent of time: 1 Δ = T E

or

T =E

Δ .

Some materials, called viscoelastic, feature a time-dependent stress-strain relation. We will not discuss them here. We will therefore restrict discussion to elastic materials and their mechanical behavior in the elastic range.

13.2. Compliance and stiﬀness tensors 13.2.1. Generalized Hooke’s law As we just saw, Young’s modulus is not suﬃcient to characterize the elastic deformation of a bar, since its cross section decreases at the same time as it elongates. Furthermore, we are interested in crystals, and thus in anisotropic materials. We also want to be able to deal with stresses that are not necessarily uniaxial. Hooke’s law must then be generalized. It relates the stress tensor Tij to the strain tensor Sij : Sij = sijkl Tkl .

(13.1a)

Conversely, the stress tensor is related to the strain tensor by relation: Tij = cijkl Skl .

(13.1b)

The coeﬃcients sijkl are called the compliance constants, and the coeﬃcients cijkl the stiﬀness constants.2 Relations (13.1a) and (13.1b) each represents a set of 9 equations which relate the components of a rank-2 tensor ([T ] or [S]) to the components of another rank-2 tensor ([S] or [T ]) through coeﬃcients sijkl or cijkl , which are therefore the components of rank-4 tensors (see Sect. 9.4.2), the compliance tensor [s] for sijkl and the stiﬀness tensor [c] for cijkl . It may be useful to show this in this special case for one of the two tensors, sijkl for example. In a change of orthonormal axis system, Sij becomes Smn and Tkl becomes Tpq such that (Eq. (9.13a) and (9.13b)): = ami anj Sij , Smn Tkl = apk aql Tpq

where {aij } is the transformation matrix from the old to the new axis system. We obtain: = ami anj sijkl Tkl = ami anj sijkl apk aql Tpq Smn

2. The sijkl and cijkl are sometimes called elastic moduli and elastic constants respectively.

Chapter 13 – Elasticity so that

263

= smnpq Tpq Smn

with

smnpq = ami anj apk aql sijkl

(13.2)

i.e. a transformation identical to that of the product of four components. This proves that sijkl is a rank-4 tensor. We can rewrite relations (13.1a) and (13.1b) in the form: [S] = [s][T ], [T ] = [c][S], where [s] is the compliance tensor and [c] the stiﬀness tensor. Since the strain tensor [S] is dimensionless, the components of [s] are dimensionally the inverse of a stress, i.e. m2 N−1 . Typical orders of magnitude for the compliance tensor components are 10−11 m2 N−1 . The stiﬀness tensor components cijkl are expressed in N m−2 and have values on the order of 1011 N m−2 . Example: the central part of the tensile specimen of Figure 13.1 is submitted to a uniform uniaxial stress represented by tensor ⎞ ⎛ T 0 0 ⎝ 0 0 0 ⎠ 0 0 0 in an axis system (Ox1 x2 x3 ) where Ox1 is parallel to the specimen axis. The generalized Hooke’s law (Eq. (13.1a)) provides, for the diagonal components: S11 = s1111 T,

S22 = s2211 T

and

S33 = s3311 T

since only T11 = T is non-zero. These components represent the (algebraic) relative elongations along the specimen axis (S11 ) and perpendicular to it (S22 and S33 ). The two latter components have no reason to be equal, in contrast to the isotropic case. The terms obtained for i = j, Sij = sij11 T , represent shear strains.

13.2.2. Symmetry of the compliance and stiﬀness tensors We saw that the stress tensor is symmetric (Sect. 11.4). We can therefore, in relation (13.1a), collect the terms containing components Tkl and Tlk for which k is diﬀerent from l. The strain Sij thus takes the form: (sijkl + sijlk )Tkl . Sij = sijkk Tkk + kl=23,31,12

Therefore sijkl and sijlk cannot be distinguished, and they are chosen equal: sijkl = sijlk .

264

Symmetry and Physical Properties of Crystals

In the same way, since Sij = Sji (Sect. 12.2.3), we have sijkl = sjikl . Thus sijkl = sijlk = sjikl = sjilk . For the same reasons, we also have: cijkl = cijlk = cjikl = cjilk . These symmetry relations reduce the number of independent components of [s] and [c] from 81 to 36. There are 9 diﬀerent ij-couples, and the same applies for the kl, thus in total 81 diﬀerent values for ijkl. Among the ij (or kl) couples, 3 are such that i = j and 6 are such that i = j. Symmetry with respect to i and j cancels 3 of the latter 6 couples, which brings to 6 instead of 9 the number of ij couples giving independent values of sijkl . The same applies for the kl couples. There remain in total 6 × 6 = 36 components of sijkl (and cijkl ) which are independent. We will see that thermodynamic arguments further reduce the number of components, which goes down to 21 because of symmetry with respect to ij and kl: sijkl = sklij and cijkl = cklij .

13.3. Contracted notation (Voigt’s notation) Because of the symmetry properties of tensor sijkl and cijkl , their expression can be simpliﬁed by replacing each couple ij (and kl) by a single subscript, denoted α for ij and β for kl, α and β ranging from 1 to 6. The correspondence is given in Table 13.1. Table 13.1: Equivalence between subscripts ij (or kl) and α (or β) ij or kl

11

22

33

2 3 and 3 2

3 1 and 1 3

1 2 and 2 1

α or β

1

2

3

4

5

6

The same simpliﬁcation makes it possible to replace the Tij and the Sij by Tα and Sα components (α ranging from 1 to 6). It is however necessary to be careful about the way these replacements are performed.

13.3.1. Stress tensor We set Tα = Tij = Tji . The tensor then takes the form: ⎛

⎞ T1 T6 T5 ⎝ T6 T2 T4 ⎠ . T5 T4 T3

(13.3)

Chapter 13 – Elasticity

265

13.3.2. Strain tensor We set: Sα = Sij

if i = j

and

Sα = Sij + Sji

if i = j.

(13.4)

The strain tensor thus has the form: ⎛ ⎞ S1 S6 /2 S5 /2 ⎝ S6 /2 S2 S4 /2 ⎠ . S5 /2 S4 /2 S3 The contracted form makes it possible to represent these two tensors in the form of column vectors with six components, Tα and Sα . We will see in the following section that the beneﬁt of using diﬀerent relations to go over from the 2-subscript notation to the single subscript notation is that the column vectors Sα and Tα are connected by a matrix relation: Sα = sαβ Tβ , and conversely Tα = cαβ Sβ .

13.3.3. Compliance tensor and stiﬀness tensor This section shows how to go over from tensors sijkl and cijkl to their simpliﬁed form sαβ and cαβ respectively. We start out by evaluating S1 = S11 = s11kl Tkl as a function of the Tα , deﬁned in Section 13.3.1: S1 = s1111 T1 + s1122 T2 + s1133 T3 + (s1123 + s1132 )T4 + (s1131 + s1113 )T5 + (s1112 + s1121 )T6 . Using the symmetry of the sijkl (Sect. 13.2.2), we set s11 = s1111 ,

s12 = s1122 ,

s13 = s1133 ,

s14 = 2s1123 ,

s15 = 2s1131 ,

s16 = 2s1112 .

We can now write: S1 = s1α Tα . The same argument applies to S2 and S3 . Now we evaluate S23 and S32 , and then add them: S23 = s2311 T1 + s2322 T2 + s2333 T3 + (s2323 + s2332 )T4 + (s2331 + s2313 )T5 + (s2312 + s2321 )T6 , S32 = s3211 T1 + s3222 T2 + s3233 T3 + (s3223 + s3232 )T4 + (s3231 + s3213 )T5 + (s3212 + s3221 )T6 . Since we set S4 = S23 + S32 , we can write: S4 = s4α Tα if we set:

s41 = 2s2311 ,

s42 = 2s2322 ,

s43 = 2s2333 ,

s44 = 4s2323 ,

s55 = 4s3131 ,

s66 = 4s1212 .

266

Symmetry and Physical Properties of Crystals

Thus we can write: Sα = sαβ Tβ providing we set: sαβ = sijkl sαβ = 2 sijkl

for α and β equal to 1, 2 or 3 (i = j and k = l), when either of the two subscripts α or β is equal to 1, 2 or 3 and the other one is equal to 4, 5 or 6, for α and β equal to 4, 5 or 6.

sαβ = 4 sijkl

We can summarize the above results by splitting Table 13.2, consisting of 9 × 9 coeﬃcients sijkl , into 9 tables with 3 rows and 3 columns each. Table 13.2: Splitting the 9×9 table of components sijkl into a set of 3×3 tables ij kl

11

22

33

23

31

12

32

13

21

11 22

I

II

III

IV

V

VI

VII

VIII

IX

33 23 31 12 32 13 21 The (6×6) matrix of coeﬃcients sαβ is obtained by superimposing and adding the sectors of the third large column to the sectors of the second large column, and then performing the same operation (superimposing, then adding) for the second and third large rows thus obtained. We ﬁnally obtain the condensed Table 13.3. Now we ﬁnd the relations between components cijkl and cαβ that allow writing Tα = cαβ Sβ . By deﬁnition, Tα = Tij = Tji , and relation (13.1b) has the form: Tα = Tij = cij11 S11 + cij22 S22 + cij33 S33 + cij23 S23 + cij32 S32 + cij31 S31 + cij13 S13 + cij12 S12 + cij21 S21 .

Chapter 13 – Elasticity

267

Table 13.3: Condensed form of the table of components sαβ α

1 2

β

3

4 5

6

1 2

I

II + III

3 4

V + VI

5

IV + VII

+

6

VIII + IX

Because of the symmetry with respect to k and l of components cijkl : Tα = Tij = cij11 S11 + cij22 S22 + cij33 S33 + cij23 (S23 + S32 ) + cij31 (S31 + S13 ) + cij12 (S12 + S21 ) and, taking into account the deﬁnition (13.4) of the Sα : Tα = cαβ Sβ if we set cαβ = cijkl . The table of the cαβ is now obtained starting from the table of cijkl by simply canceling the sectors that form the third large column and the third large row (Tab. 13.4). The components cαβ and sαβ each form a square 6 × 6 matrix. Table 13.4: Condensed form of the table of stiﬀness components cαβ . The gray areas are canceled. α β

1 2 3

4 5 6

I

II

IV

V

1 2 3 4 5 6

268

Symmetry and Physical Properties of Crystals

13.3.4. Relation between the compliance and stiﬀness tensors Using the simpliﬁed notation we just introduced, the generalized Hooke’s law can be written in the following matrix form: Sα = sαβ Tβ , Tα = cαβ Sβ . These relations show that matrices sαβ and cαβ , which we note here s and c, are mutually inverse: sc = E where E is the identity matrix. To calculate the stiﬀness components cαβ starting from the compliance components sαβ , it is suﬃcient to invert the compliance matrix, and vice versa. To conclude, the simpliﬁed notation we just introduced allows representing the stress → strain (and conversely strain → stress) relation by a matrix relation where the rank-2 tensors (stress and strain) become six-component column vectors, and the rank-4 tensors (compliance and stiﬀness) become 6 × 6 square matrices. Matrices s and c represent a simpliﬁed form of tensors sijkl and cijkl , expressed in a given coordinate system. If we want to know the expression of these matrices in another coordinate system, we have to revert to the four-subscript components of tensors sijkl and cijkl , then perform the change in axis system on these components (Eq. (13.2)), and ﬁnally revert again to the contracted form of the new components sijkl and cijkl thus obtained.

13.4. Energy of a strained solid Consider a small volume of crystal which, before deformation, has the shape of a rectangle parallelepiped. Choose a reference system consisting of orthonormal axes Ox1 x2 x3 , parallel to its sides, with lengths respectively Δx1 , Δx2 and Δx3 (Fig. 13.3). We submit it to a stress, described by the tensor Tkl which induces the strain Sij . Then we increase this deformation by a small quantity dSij . We now show that the elementary work of the stress forces during this change in deformation has the form δW = Tij dSij ΔV if ΔV is the volume of the parallelepiped. After deformation, the faces of the parallelepiped are not exactly rectangles with the same area any more, but, since the deformations are assumed to be very small, we can consider that the change in area of the faces is negligible and that the faces remain perpendicular to the coordinate axes. If the parallelepiped had been only translated without undergoing a strain, the work of the stress forces would be zero since the forces acting on two opposite faces are equal and have opposite directions. Thus the work is due only to the relative displacement of one face with respect to the other. We may

Chapter 13 – Elasticity

269

therefore, for calculation purposes, assume that the three parallelepiped faces which go through the origin remained ﬁxed, and that the work is due to the displacement of the three opposite faces. Consider the face perpendicular to axis Ox1 . It gets displaced because of the components dS11 , dS21 and dS31 of tensor dSij , which represent the relative deformation of a segment parallel to Ox1 . Term dS11 describes a displacement of this face parallel to Ox1 by Δx1 dS11 (Fig. 13.3a). During this displacement, only the component T11 of the stress tensor performs work, equal to T11 Δx2 Δx3 Δx1 dS11 = T11 dS11 ΔV . The strain component dS21 leads to a displacement of this face parallel to Ox2 by Δx1 dS21 (Fig. 13.3b), and only the component T21 performs work, equal to T21 Δx2 Δx3 Δx1 dS21 = T21 dS21 ΔV . In the same way, the strain dS31 leads to a displacement parallel to Ox3 of the face, and only the component T31 does work, equal to T31 dS31 ΔV . x3

x3

x3 O

O

x2

x2

x1 x1

x1dS11

x2

x1

x2

(a)

x1dS21

(b)

Figure 13.3: (a) Displacement parallel to Ox 1 of the face perpendicular to Ox 1 of the rectangle parallelepiped under the inﬂuence of component dS 11 of the strain tensor; (b) displacement parallel to Ox 2 of the same face under the inﬂuence of component dS 21 of the strain tensor The total work of the forces acting on the faces perpendicular to Ox1 is therefore: δW1 = Ti1 dSi1 ΔV. We would obtain in the same way the works δW2 and δW3 of the forces acting respectively on the faces perpendicular to Ox2 and Ox3 : δW2 = Ti2 dSi2 ΔV,

δW3 = Ti3 dSi3 ΔV.

The total work δW per unit volume of the material is then equal to: δW = (δW1 + δW2 + δW3 )/ΔV

or

δW = Tij dSij

(13.5)

or, in detailed form: δW = T11 dS11 + T22 dS22 + T33 dS33 + T23 dS23 + T32 dS32 + T31 dS31 + T13 dS13 + T12 dS12 + T21 dS21 .

270

Symmetry and Physical Properties of Crystals

Using relations (13.3) and (13.4) which deﬁne the Tα and the Sα components, we see that: δW = Tα dSα and, since Tα = cαβ Sβ , we can write the above relation in the form: δW = cαβ Sβ dSα . The work we just calculated is reversible work, because a small variation in strain with all of its components dSα equal and opposite to the above variation would take the system back to its initial state. The variation dF in the free energy F = U − ΘS per unit volume is such that: dF = dU − ΘdS − SdΘ = δW + δQ − ΘdS − SdΘ where S it the entropy and Θ the absolute temperature. For a reversible transformation: δQrev = ΘdS

and

dF = δWrev − SdΘ

so that dF = cαβ Sβ dSα − SdΘ. We deduce that: cαβ

(13.6)

∂ 2 F ∂ 2 F = = = cβα . ∂Sβ ∂Sα Θ ∂Sα ∂Sβ Θ

The cαβ are thus the stiﬀness coeﬃcients at constant temperature, and this relation shows that the matrix of cαβ coeﬃcients is symmetric. Therefore, the stiﬀness tensor cijkl is symmetric with respect to its two subscript groups ij and kl: cijkl = cklij . A similar argument using the thermodynamic function Φ, the Gibbs potential or free enthalpy, such that Φ = U − ΘS − Tα Sα , provides the same results for the compliance tensor. We have dΦ = −SdΘ − Sα dTα = −SdΘ − sαβ Tβ dTα and sαβ = −

∂ 2 Φ ∂ 2 Φ = − = sβα . ∂Tβ ∂Tα Θ ∂Tα ∂Tβ Θ

The sαβ are the compliance components at constant temperature and furthermore: or sijkl = sklij . sαβ = sβα These relations bring down to 21 the maximum number of independent components of the elastic and stiﬀness tensors.

Chapter 13 – Elasticity

271

The variation in free energy dF at constant temperature (dΘ = 0) takes the form, using (13.6): dF = cαα Sα dSα + cαβ (Sα dSβ + Sβ dSα ) α

=

αβ=23,31,12

cαα Sα dSα +

α

cαβ d(Sα Sβ ).

αβ=23,31,12

We obtain after integration: F=

1 α

=

2

cαα Sα2 +

cαβ Sα Sβ

αβ=23,31,12

1 1 cαα Sα2 + cαβ Sα Sβ . 2 α 2 α=β

Thus the elastic free energy per unit volume of a strained solid is given by: F =

1 cαβ Sα Sβ . 2

The above derivations were made using the expression of elementary work δW = Tα dSα . They could also have been made using the unsimpliﬁed forms of the tensors, δW = Tij dSij . We would then have obtained cijkl = cklij and sijkl = sklij , and for the free energy: F =

1 cijkl Sij Skl . 2

13.5. Eﬀect of crystal symmetry on the form of the elastic tensor We will use the direct inspection method (Sect. 9.6.2) to determine the number of independent components of the elastic (or stiﬀness) tensor for some point groups. The results for all point groups are collected in Tables 13.5a and 13.5b. Because the matrices sαβ and cαβ are symmetric, the part of the matrix deduced by symmetry is not represented. We recall that, in order to use the direct inspection method or the coordinate system change formula, we must revert to the four-subscript tensor notation.

272

Symmetry and Physical Properties of Crystals

Table 13.5a: Form of the matrices representing the compliance and stiﬀness tensors for the various point groups Triclinic

Monoclinic 2 Ox 2 m Ox 2

0 0 0

0 0 0 0

2 Ox 3 m Ox 3

0

Orthorhombic

0 0 0 0 0 0 0 0 0 0 0 0

Tetragonal

0 0 0 0 0 0 0 0 0 0

4 – 4 4/m

422 4mm – 42m 4/mmm

Equal components Components with equal absolute values but opposite signs

0 0 0 0 0 0 0 0

0 0 0 0 0 0 0 0 0 0 0 0

Chapter 13 – Elasticity

273

Table 13.5b: Form of the matrices representing the compliance and stiﬀness tensors for the various point groups Rhombohedral

3 – 3

0 0 0 0 0 0

32 3m – 3m

* Hexagonal

0 0 0 0 0

0 0 0 0

*

0 0 0 0 0 0 0 0 0 0 0 0

* Cubic

0 0 0 0 0 0 0 0 0 0 0 0

Isotropic

0 0 0 0 0 0 0 0 0 * 0 0 * 0

* Equal components Components with equal absolute values but opposite signs For s : value twice that of the component shown as a full circle to which it is connected For c : value equal to the component shown as a full circle to which it is connected

*

For s : 2(s11 – s12) For c : 1/2(c11 – c12)

274

Symmetry and Physical Properties of Crystals

13.5.1. Center of symmetry Tensors [s] and [c] being even-rank tensors, the existence or non-existence of a center of symmetry among the point symmetry operations of the crystal does not alter the number of independent components of these tensors (see Sect. 9.6.3). Thus, the number of independent components for these tensors is the same for all point groups of a given Laue class.

13.5.2. Groups 2, m and 2/m We choose axis Ox3 parallel to the 2-fold axis. Rotating the coordinate system by π around the 2-fold axis transforms components x1 , x2 , x3 of a vector into components x1 , x2 , x3 such that: x1 = −x1 ,

x2 = −x2 ,

x3 = x3 .

We deduce that the components sijkl whose subscripts i, j, k, l contain an odd total number of 1 and 2’s and, consequently, an odd number of 3’s, are zero. The tensors [s] and [c] shown in their condensed form {sαβ } or {cαβ } reduce to: 0 0 0 0 0 0 0 0

We obtain the same result by considering group m and axis Ox3 perpendicular to the mirror. The symmetry operation acting on the coordinate system changes the components x1 , x2 , x3 of a vector into components x1 , x2 , x3 such that: x1 = x1 ,

x2 = x2 ,

x3 = −x3 ,

so that any component of sijkl (or cijkl ) involving an odd number of 3’s is zero. This result is also valid for group 2/m, as expected since adding a mirror perpendicular to the 2-fold axis does not reduce the number of non-zero coefﬁcients. It is no surprise to obtain the same result for groups 2, m and 2/m since they belong to the same Laue class.

13.5.3. Groups 222, mmm and mm2 These three groups, which belong to the same Laue class, have the same number of independent coeﬃcients, and we will only consider group 222. It has three mutually perpendicular 2-fold axes, which we choose as the axes Ox1 , Ox2 and Ox3 . We use the results of the preceding section for the 2-fold axis parallel to Ox3 , and we add the symmetry operation associated to the 2-fold

Chapter 13 – Elasticity

275

axis parallel to Ox1 , a rotation by π of the coordinate system around Ox1 . This operation transforms the components x1 , x2 , x3 of a vector into components x1 , x2 , x3 such that x1 = x1 ,

x2 = −x2 ,

x3 = −x3 .

All components involving an odd total number of subscripts equal to 1 are zero. We need not consider the action of the third 2-fold axis, because its existence results from the existence of the two others. We therefore obtain the following matrix: 0 0 0 0 0 0 0 0 0 0 0 0

13.5.4. Groups 422, 4mm and 4/m mm Each of these groups belongs to the same Laue class and can be deduced from one of the above by replacing a 2-fold axis with a 4-fold axis. For these three groups, axis Ox3 is chosen parallel to the 4-fold axis. This substitution adds a symmetry operation, the rotation by π/2 around Ox3 . This operation, performed on the axis system, transforms components x1 , x2 , x3 of a vector into components x1 , x2 , x3 such that: x1 = x2 ,

x2 = −x1 ,

x3 = x3 .

We deduce that: s1111 = s2222 ,

s1133 = s2233

and s1313 = s2323 .

We ﬁnally obtain the following matrix, where lines connecting some dots indicate that the corresponding coeﬃcients are equal: 0 0 0 0 0 0 0 0 0 0 0

This result is also valid for group ¯42m, which belongs to the same Laue class.

276

Symmetry and Physical Properties of Crystals

13.5.5. Cubic system The least symmetric among the cubic groups is group 23. It has three orthogonal 2-fold axes parallel to the cube sides, and four 3-fold axes parallel to its major diagonals. We can therefore start from the number of independent coeﬃcients determined for group 222 in a system of axes parallel to the 2-fold axes, and add a 3-fold axis, for example the axis parallel to direction [111]. A rotation by 2π/3 around this 3-fold axis, performed on the axis system, transforms the components x1 , x2 , x3 of a vector into components x1 , x2 , x3 such that: x1 = x2 ,

x2 = x3 ,

x3 = x1 .

We deduce that: s1111 = s2222 = s3333

and also s1122 = s2233 = s3311 etc.

We ﬁnally obtain the following matrix: 0 0 0 0 0 0 0 0 0 0 0 0

We then check that the additional symmetries in the other cubic groups bring no further simpliﬁcation. Thus only 3 independent coeﬃcients are involved in describing the elasticity of cubic crystals. The order of magnitude of the sαβ is some 10−11 m2 N−1 , that of the cαβ some 1011 N m−2 . Some numerical values of components sαβ and cαβ are given in Tables 13.6a and 13.6b respectively.

13.6. Isotropic materials We saw, in the introduction to this chapter, that only 2 coeﬃcients are required to describe the elastic properties of isotropic materials: Young’s modulus E, and Poisson’s ratio ν. Here we will establish the connection between these coeﬃcients E and ν and the components of the compliance and stiﬀness tensors. The compliance tensor (as well as the stiﬀness tensor) of an isotropic material must be invariant under any change in coordinate system. A simple way of expressing this condition is to start from tensor sijkl for a cubic material, and to perform any change in the coordinate system (for example a rotation by π/4

Chapter 13 – Elasticity

277

Table 13.6a: Numerical values of the compliance coeﬃcients sαβ for some materials (unit: 10−11 m2 N−1 ) 11

12

44

1.5

−0.63

1.32

0.77

−0.22

1.26

2.29

−0.47

7.85

Co

6/mmm 0.47

−0.23

Ti

6/mmm 0.97

−0.47

SiC

6/mmm 0.21

−0.037 0.59

−0.017 0.18

Crystal Cu Si NaCl

P.G. ¯ m3m ¯ m3m ¯ m3m

13

33

1,32

−0.07

0.32

2.15

−0.18

0.69

14

1.10

−0.46

3.45

−0.21

Al2 O3

6mm ¯3m

0.24

−0.07

0.7

−0.038 0.22

0.049

LiNbO3

3m

0.57

−0.09

1.67

−0.15

0.49

−0.1

Quartz (SiO2 )

32

1.17

−0.08

1.72

−0.12

0.97

−0.39

KDP

¯42m

1.49

0.18

7.69

−0.39

1.97

ZnS

66

0.85

16.7

Table 13.6b: Numerical values of the stiﬀness coeﬃcients cαβ for some materials (unit: 1011 N m−2 ) 11

12

44

13

33

1.69

1.22

0.75

1.65

0.64

0.79

0.49

0.13

0.13

Co

6/mmm 3.07

1.65

0.75

1.03

3.58

Ti

6/mmm

1.6

0.9

0.46

0.66

1.81

SiC

6/mmm

5

1

1.7

0.6

5.6

ZnS Al2 O3

6mm ¯3m

1.24

0.6

0.29

0.46

1.4

4.95

1.6

1.46

1.15

4.97

−0.23

LiNbO3

3m

2.03

0.53

0.6

0.75

2.45

0.09

Quartz (SiO2 )

32

0.87

0.07

0.58

0.12

1.06

0.18

KDP

¯42m

0.71

−0.05

0.13

0.13

0.56

Crystal Cu Si NaCl

P.G. m¯3m m¯3m m¯3m

14

66

0.06

278

Symmetry and Physical Properties of Crystals

around a 4-fold axis parallel to one of the axes Ox1 , Ox2 or Ox3 ). This must leave all the tensor coeﬃcients unchanged (Exercise 13.2). We thus obtain the result that, for an isotropic material, the three independent components of the compliance and stiﬀness tensors which characterize the cubic system are connected by the following relations: s44 = 2(s11 − s12 ), c44 =

1 2 (c11

(13.7a)

− c12 ).

(13.7b)

This is of course valid whatever the orthonormal coordinate system used. There are thus only 2 independent elastic components for isotropic solids. They are expressed as a function of E and ν in the following section. We note here that cubic materials are diﬀerent from isotropic materials as far as elastic properties are concerned. This is a general result for all physical properties represented by rank-4 crystals. In contrast, for the properties represented by rank-2 tensors, cubic materials behave as isotropic (Sect. 10.5.5). The deviation from isotropy of the elastic properties of cubic materials can be evaluated by comparing the values of c44 and 12 (c11 − c12 ), or the values of s44 and 2(s11 − s12 ).

13.6.1. Expressing components sαβ as a function of E and ν Consider a tensile specimen of an isotropic material, undergoing an elongation under the inﬂuence of a uniaxial stress T . We choose Ox1 parallel to the axis of the specimen and to the stress (Fig. 13.1). The strain is obtained through the generalized Hooke’s law: ⎞ ⎛ ⎞⎛ ⎞ ⎛ ⎞ ⎛ 0 0 s11 s12 s12 0 T S1 s11 T ⎟ ⎜ ⎜ S2 ⎟ ⎜ s12 s11 s12 0 ⎟ ⎜ 0 0 ⎟ ⎟ ⎜ ⎟ ⎜ 0 ⎟ ⎜ s12 T ⎟ ⎜ ⎟ ⎜ 0 ⎟ ⎜ s12 T ⎟ ⎜ S3 ⎟ ⎜ s12 s12 s11 0 0 0 ⎟ ⎜ ⎟⎜ ⎟. ⎜ ⎟=⎜ ⎟ ⎜ ⎜ S4 ⎟ = ⎜ 0 ⎟ ⎜ 0 ⎟ 0 0 s44 0 ⎟ ⎜ ⎟⎜ 0 ⎟ ⎜ 0 ⎟ ⎜ ⎠ ⎝ ⎝ S5 ⎠ ⎝ 0 ⎠ ⎝ 0 0 0 s44 0 0 ⎠ 0 S6

0

0

0

0

0

s44

0

0

Also, s44 = 2(s11 − s12 ) according to (13.7a). The bar thus undergoes a relative elongation S1 = Δ/ = s11 T , and we deduce that s11 = 1/E where E is Young’s modulus for the material. Along with this elongation, the bar undergoes the same deformation in the two directions perpendicular to the stress: S2 = S3 = s12 T . From the deﬁnition of Poisson’s ratio ν, as given in the introduction, we see that: s12 = −ν s11 so that s12 = −

ν . E

Chapter 13 – Elasticity

279

Hence: s44 = 2

ν 1 + E E

=

2(1 + ν) . E

The shear (or rigidity) modulus G is deﬁned as the reciprocal of s44 , i.e. as the ratio of a shear stress and the corresponding shear strain, so that: G=

E 1 . = c44 = s44 2(1 + ν)

13.6.2. Stiﬀness components. Lamé coeﬃcients For isotropic materials, the stiﬀness components are not much used in the form of the cαβ . It is customary to use the Lamé coeﬃcients, λ and μ, deﬁned as follows: c44 = μ and c12 = λ and, using (13.7b): c11 = 2c44 + c12 = λ + 2μ. The stiﬀness tensor can thus be written as: ⎛ λ + 2μ λ λ ⎜ λ λ + 2μ λ ⎜ ⎜ λ λ λ + 2μ ⎜ ⎜ 0 0 0 ⎜ ⎝ 0 0 0 0 0 0

0 0 0 μ 0 0

0 0 0 0 μ 0

0 0 0 0 0 μ

⎞ ⎟ ⎟ ⎟ ⎟. ⎟ ⎟ ⎠

Hooke’s generalized law (Eq. (13.1b)) now takes the form: for α = 1, 2, 3 : and for α = 4, 5, 6 :

Tα = 2μSα + λ(S1 + S2 + S3 ), Tα = μSα .

Since Sα = Sij for α = 1, 2, 3 and Sα = Sij + Sji = 2Sij for α = 4, 5, 6, these two relations can be condensed into a single one: Tij = 2μSij + λ(Trace S)δij .

13.7. Representative surface for Young’s modulus It is often valuable to ﬁnd how the length of a bar of an anisotropic material, with known but general crystallographic direction, changes when it is submitted to a uniaxial stress parallel to the bar, i.e. the equivalent of Young’s modulus for an isotropic material. We deﬁned Young’s modulus Ew in a given direction with unit vector w as the ratio between the value T of a uniaxial stress in this direction and the relative elongation Δ/|w of the material in the same direction, Ew = T /( Δ/|w ). Choosing an orthonormal axis system (Ox1 x2 x3 ) where Ox1 is parallel to vector w, the stress tensor has only one non-zero component in this coordinate

280

Symmetry and Physical Properties of Crystals

= T . The relative elongation in direction Ox is given by S , system, T11 1 11 so that: Δ = S11 = s1111 T w

where s1111 is the compliance component expressed in the axis system (Ox1 x2 x3 ). We deduce that: 1 Ew = . s1111 We thus have to calculate s1111 as a function of the independent components sijkl of the compliance tensor in the orthonormal axis system Ox1 , Ox2 and Ox3 associated to the crystallographic system. The rule for axis system change provides: s1111 = a1i a1j a1k a1l sijkl where {aij } is the transformation matrix for going over from coordinate system (Ox1 x2 x3 ) to system (Ox1 x2 x3 ). The only coeﬃcients of the matrix actually involved are the a1j , i.e. the components of the new basis vector e1 , which is none other than vector w, in the frame Ox1 x2 x3 . These are the direction cosines of w in this frame. They are noted w1 , w2 , w3 , yielding: s1111 = wi wj wk wl sijkl . The representative surface for Young’s modulus is deﬁned as the locus of the ends of vectors starting from the same origin, with lengths in a given direction w equal to the corresponding value s1111 . This surface thus represents the reciprocal of Young’s modulus for any direction of the applied uniaxial stress. Example for the cubic system: s11 = s11 w14 + w24 + w34 + s44 w22 w32 + w32 w12 + w12 w22 + 2s12 w22 w32 + w32 w12 + w12 w22 . Since w is a unit vector, we have:

2 w14 + w24 + w34 = w12 + w22 + w32 − 2 w22 w32 + w32 w12 + w12 w22 = 1 − 2 w22 w32 + w32 w12 + w12 w22

s44 2 2 w2 w3 + w32 w12 + w12 w22 . s11 = s11 − 2 s11 − s12 − 2 Thus Young’s modulus is not isotropic for cubic crystals. and

For direction [100], s11 = s11 , while for direction [111], we obtain: s11 = s11 − 2/3 (s11 − s12 − s44 /2). It can be shown that this value is extremal (Exercise 13.5). Note: in an isotropic material, s11 − s12 = s44 /2, and, as expected, 1/E = s11 for any direction.

Chapter 13 – Elasticity

281

13.8. Compressibility Two types of compressibility at constant temperature can be deﬁned depending on whether interest focuses, for a solid submitted to a pressure variation Δp, on the change in volume or on the change in length in a given direction. In either case, the pressure variation Δp induces a variation of the stress tensor ΔTij = −δij Δp which leads to a strain variation ΔSij such that: ΔSij = sijkl ΔTkl = −sijkl δkl Δp = −sijkk Δp

(13.8)

13.8.1. Bulk compressibility The bulk compressibility coeﬃcient χ at constant temperature Θ is deﬁned by:

1 ∂V χ=− . V ∂p Θ If ΔV is a small variation in the volume V of the material caused by a small pressure variation Δp at constant temperature:

1 ΔV χ=− . Δp V We saw (Sect. 12.4) that the relative volume variation is such that: ΔV = Sii V and, because of Equation (13.8): ΔV = −siikk Δp. V Thus

1 χ=− Δp

ΔV V

= siikk

i.e. the sum of the nine coeﬃcients in the ﬁrst quarter of matrix sαβ : χ = [s11 + s22 + s33 + 2(s12 + s23 + s31 )]. In the case of an isotropic material, this relation becomes: χ = 3[s11 + 2s12 ] and, since s11 = 1/E and s12 = −ν/E, we obtain:

1 − 2ν χ=3 . E

282

Symmetry and Physical Properties of Crystals

Its reciprocal K is called the bulk modulus: K=

E 1 = . χ 3(1 − 2ν)

K and χ are positive quantities, since when the pressure applied on a solid is increased, its volume decreases: ΔV /V < 0. Thus for all materials ν < 1/2. It can also be shown [1] that the Lamé coeﬃcient μ is always positive. If E is expressed as a function of μ and ν in the expression for K, we obtain: K=

2 μ(1 + ν) 3 (1 − 2ν)

whence:

1 −1 < ν < . 2 In practice, a negative value of ν is exceptional, but it was encountered [2]. For most polycrystalline metals, described as isotropic materials, ν is on the order of 0.3.

13.8.2. Linear compressibility of a bar The linear compressibility coeﬃcient at constant temperature in a given direction w of a material, βw , is deﬁned by:

1 ∂ βw = − ∂p Θ which can be written: βw = −

1

Δ Δp

=−

1 Δp

Δ

if Δp is a small pressure variation, at constant temperature, which induces a small variation in length Δ in a segment with length parallel to vector w. We saw (Eq. (12.12)) that the relative elongation of such a segment, submitted to a variation in the strain tensor ΔSij , is given by: Δ = wi wj ΔSij w and, using Equation (13.8): Δ = −wi wj sijkk Δp. w Hence the linear compressibility coeﬃcient at constant temperature is given by: βw = wi wj sijkk .

Chapter 13 – Elasticity

283

13.9. Notes on non-uniform stresses and strains We saw in Section 11.5 that it is necessary, in order to determine tensor Tij (r) in a material submitted to given stresses (Tn )Σ on its external surface Σ, to solve Equations (11.4) ∂Tij + fi = 0, (11.4) ∂xj at all points in the solid, with the boundary conditions: (Tn )Σ = (Tij )Σ (nj )Σ .

(13.9)

We must therefore determine a tensor [T ] satisfying (11.4) and (13.9). Since tensor [T ] is related to tensor [S] through Hooke’s law [T ] = [c][S], condition (11.4) leads to a condition on the derivatives of [S]. But the six components of the symmetric tensor [S] cannot take any value in the case of non-uniform strains, because they are expressed as a function of the derivatives of the three components of the displacement vector u. Consider for example the components S11 , S22 and S12 which imply functions u1 and u2 . By deﬁnition:

∂u1 ∂u2 1 ∂u1 ∂u2 S11 = S22 = S12 = + . ∂x1 ∂x2 2 ∂x2 ∂x1 We immediately see that these three quantities are not independent. The second derivative of S12 with respect to x1 and x2 has the form:

3 ∂ 3 u2 ∂ u1 1 + 2 ∂x1 ∂x22 ∂x2 ∂x21 thus the half-sum of

∂ 2 S11 ∂x22

and

∂ 2 S22 . ∂x21

We must therefore have: 2

∂ 2 S11 ∂ 2 S22 ∂ 2 S12 = + . ∂x1 ∂x2 ∂x22 ∂x21

(13.10)

It can be shown that there are six such compatibility relations. Further, since the basic relation (11.4) must be veriﬁed, one way of incorporating the compatibility relations is to substitute, in these equations, the Sij by their expression as a function of the Tij , and to add condition (11.4). We then obtain six coupled equations, called the Beltrami-Michell equations. They can usually not be solved analytically, and their solution is obtained numerically. Another way of translating Equation (11.4) is to replace in this equation the stresses by their expression as a function of the Sij , and then to express the Sij as a function of the derivatives of displacement u. The calculation is easy in the isotropic case.

284

Symmetry and Physical Properties of Crystals

Relation (11.4) for i = 1 can be written, in the isotropic case: ∂T1j + f1 = 0 ∂xj

∂T1 ∂T6 ∂T5 + + + f1 = 0. ∂x1 ∂x2 ∂x3

or

(13.11)

Hooke’s law Tα = cαβ Sβ can we written, using the Lamé coeﬃcients (Sect. 13.6.2), as: T1 = 2μS1 + λ(S1 + S2 + S3 ), T5 = μS5 , T6 = μS6 and Equation (13.11) becomes:

∂S1 ∂S6 ∂S5 ∂S1 ∂S2 ∂S3 μ 2 +λ + f1 = 0. + + + + ∂x1 ∂x2 ∂x3 ∂x1 ∂x1 ∂x1 Also (Eq. (12.10)): 1 Sij = 2

∂uj ∂ui + ∂xj ∂xi

(13.12)

.

Since, from Equation (13.4), S5 = S13 + S31 and S6 = S12 + S21 , S5 =

∂u1 ∂u3 + ∂x3 ∂x1

and

S6 =

∂u1 ∂u2 + . ∂x2 ∂x1

Equation (13.12) thus becomes:

2 ∂ 2 u2 ∂ 2 u1 ∂ 2 u3 ∂ u1 ∂ 2 u1 + + + μ 2 2 + ∂x2 ∂x1 ∂x3 ∂x1 ∂x1 ∂x2 ∂x23

2 2 2 2 ∂ u2 ∂ u3 ∂ u1 + f1 = 0. + + +λ ∂x1 ∂x2 ∂x1 ∂x3 ∂x21 Reorganizing the terms, we obtain: 2

2 ∂ 2 u2 ∂ 2 u3 ∂ u1 ∂ u1 ∂ 2 u1 ∂ 2 u1 + (λ + μ) + f1 = 0 μ + + + + ∂x1 ∂x2 ∂x1 ∂x3 ∂x21 ∂x22 ∂x23 ∂x21 and

μ

∂ 2 u1 ∂ 2 u1 ∂ 2 u1 + + ∂x21 ∂x22 ∂x23

+ (λ + μ)

∂ ∂u1 ∂u2 ∂u3 + + + f1 = 0 ∂x1 ∂x1 ∂x2 ∂x3

so that

∂ (div u) + f1 = 0. ∂x1 We would obtain similar relations for i = 2 and i = 3 in (11.4), so that ﬁnally: μΔu1 + (λ + μ)

μΔui + (λ + μ)

∂ (div u) + fi = 0. ∂xi

The three above relations can be collected into a single vector equation: (λ + μ)grad(div u) + μΔu + f = 0 This is Navier’s equation.

Chapter 13 – Elasticity

285

To determine the strains in the solid, we must then take into account the boundary conditions on u. In a few simple cases, the solution is analytical, but in most cases it has to be determined numerically.

13.10. Exercises Exercise 13.1 Determine the form of the elasticity tensor of a crystal with point group ¯43m by using that for a crystal with point group ¯42m given in Table 13.5a. Express it in an orthonormal axis system (Ox1 x2 x3 ) parallel to the basis vectors a, b and c of the cubic unit cell. Exercise 13.2 Consider a cubic crystal, to which an orthonormal axis system parallel to the basis vectors of the cubic unit cell is associated. 1.

It is submitted to a uniform uniaxial stress T in the [100] direction. Calculate the relative elongation in the direction of the applied stress.

2.

The uniaxial stress is now applied in the direction [110]. Calculate the relative elongation in the direction of the applied stress.

3.

If the material was isotropic, the results obtained in (1) and (2) would have to be identical. Deduce the relation which exists between the elastic coeﬃcients s11 , s12 and s44 in an isotropic material.

Exercise 13.3 A small crystal sample with volume v of tin (point group 4/m mm) is submitted to a hydrostatic stress p with value 107 N m−2 . Calculate the resulting relative variation in volume. The form of the matrix {sαβ } for this group is given in Table 13.5a, and its elements, expressed in units of 10−11 m2 N−1 , are s11 = 1.85

s12 = −0.99

s13 = −0.25

s33 = 1.18

s44 = 5.7

s66 = 13.5.

Exercise 13.4 Show that the relative variation in volume of a crystal with cubic symmetry, submitted to a uniaxial stress T , is independent of the direction of the stress and is expressed by (s11 + 2s12 )T . Exercise 13.5 Show that Young’s modulus for a cubic material is maximum in the direction [111] in all cases where s11 − s12 − s44 /2 is positive.

286

Symmetry and Physical Properties of Crystals

Exercise 13.6 A crystal of lead telluride PbTe, with point group m¯3m, is submitted to a uniform uniaxial tensile stress, with intensity 108 N m−2 , perpendicular to a (110) surface. The resulting strains are the following: a relative increase in length of 24 × 10−4 in the direction of the uniaxial stress [110], relative decreases in length along directions [001] and [1¯10], with values 6 × 10−5 and 15 × 10−4 respectively. Determine the values of the elastic coeﬃcients of PbTe. Exercise 13.7 A cubic crystal with lattice parameter a is submitted to a uniform uniaxial stress T , parallel to direction [111]. 1.

Determine the stress tensor in an orthonormal axis system (Ox1 x2 x3 ) parallel to the basis vectors of the cubic unit cell.

2.

Deduce the resulting strain tensor, in the orthonormal axis system linked to the basis vectors of the cubic unit cell.

3.

Show that the cubic unit cell becomes a rhombohedral unit cell. Calculate the lattice parameters (a = b = c and α = β = γ = π/2 − ε) as a function of the uniaxial stress T and of the elastic coeﬃcients sαβ .

Exercise 13.8 Consider test specimens made of copper, with point group m¯3m, in the shape of rectangle parallelepipeds with length L and square cross section, with side . The values are L = 5 mm, = 1 mm, and the compliance tensor components of copper are: s11 = 1.49×10−11 m2 N−1 , s12 = −0.63×10−11 m2 N−1 , s44 = 1.33 × 10−11 m2 N−1 . B

A

T

C D x

L

O x B’ A’

x

C’ D’

Assume the experimental conditions are such that the stresses to which the specimens are submitted are uniform.

Chapter 13 – Elasticity

287

1.

The ﬁrst specimen is cut so that its faces are all {100} type. The uniaxial compressive stress T is applied onto the square faces ABCD and A B C D (ﬁgure above). Determine the variation in length ΔL of the specimen, and the variation Δ of the sides of the section, for T = 109 N m−2 .

2.

Consider a second specimen, with the same dimensions as the ﬁrst one, with faces now having the following crystallographic orientations: faces ABCD and A B C D are (110) faces, faces ABB A and DCC D are (001) faces and faces ADD A and BCC B are (¯ 110) faces. The uniaxial compressive stress is applied on faces ABCD and A B C D . Determine the shape taken by the specimen, and its new dimensions.

288

Symmetry and Physical Properties of Crystals

Complement 13C. Plastic deformation and crystal defects Throughout this book, the assumption is made, for simplicity’s sake, that the crystal is perfect and has inﬁnite extension. The latter condition is obviously not to be taken literally, but the assumption of crystal perfection is also most questionable. Actually, it is only through tremendous eﬀorts that crystals of silicon are manufactured (see Complement 1C) with no defect of one kind – the linear defects called dislocations which will be discussed below. Other defects, called point defects (vacancies and interstitials) are present even in these extraordinarily good crystals, because thermodynamics requires them at equilibrium. When it comes to the discussion of X-ray or neutron diﬀraction by crystals, an introductory, geometrical treatment invokes a perfect and inﬁnite crystal in order to make the reciprocal lattice (Sect. 3.2) consist of point-like nodes. Nevertheless a discussion of the scattering mechanism and scattered intensity leads to the condition that, for the experimental results to be reasonably simple to analyze (“kinematical approximation”), the crystal must be small and imperfect. And an essential physical property of metals, mechanical ductility, is directly linked to dislocations. The macroscopic strain produced by a stress, for example in a tensile test, disappears once the applied stress is removed if the strain is small enough: this is the elastic deformation range. Under a larger stress, part of the distortion remains after the stress is removed. This is plastic deformation, and obviously it is vital for metal shaping to produce permanent eﬀects, hence in all technical activities. In terms of the macroscopic stress-strain diagram, the plastic regime starts where the curve deviates from the linear initial part (Sect. 13.1). The mechanism of plastic deformation was suggested in the 1930s to be the motion and multiplication of crystal defects called dislocation lines, or for short dislocations. This postulate was required to remove the paradox associated with the fact that plastic deformation occurs for stresses much smaller than predicted from the cohesive energy for a homogeneous crystal with no singularity. The existence of dislocations was indeed conﬁrmed through direct observation when the electron microscope was developed, and they were explored in great detail also with several other techniques, notably the X-ray imaging techniques called “diﬀraction topographic methods” or Bragg-diﬀraction imaging. A dislocation can be envisaged as the result of i) performing in an initially perfect crystal a cut ending along a line (the dislocation line); ii) moving one lip of the cut with respect to the other: the displacement deﬁnes the Burgers vector b; iii) adding or removing some perfect crystal material to ﬁll the gap or remove the overlap; iv) gluing the material together. The Burgers vector must be a lattice translation in order to allow the displaced parts to match, and it is usually, for thermodynamic reasons, the shortest lattice translation possible.

Chapter 13 – Elasticity

289 b u

v u

b v

(a)

(b)

Figure 13C.1: (a) An edge dislocation: schematic representation of the atomic planes. The Burgers vector is perpendicular to the dislocation line uv. (b) A screw dislocation. The line uv and the Burgers vector are parallel. Figure 13C.1 shows the two pure situations: in (a), the dislocation line uv is perpendicular to the Burgers vector b; this is an edge dislocation, and the plane containing the line and the Burgers vector is called the glide plane. Figure 13C.1b shows the situation where the Burgers vector b is parallel to the line uv, deﬁning a screw dislocation. In reality, dislocations usually have mixed character, i.e. their Burgers vector lies at an angle to the dislocation line. As Figure 13C.1 suggests, the lattice planes are distorted in the vicinity of the dislocation. The distortion decreases with increasing distance from the core (the center) of the dislocation. The visibility of dislocations in the electron microscope and in the Bragg-diﬀraction imaging techniques is due to the strain ﬁeld: the region with inhomogeneous distortion diﬀracts diﬀerently from the perfect-crystal matrix surrounding it. The simplest case of plastic deformation through the motion of a dislocation is illustrated in Figure 13C.2, which suggests how one part of the crystal will have moved by one Burgers vector when the dislocation line has moved across the crystal. The hatched area generated by the dislocation line is called the glide plane. Dislocations interact with one another through their stress ﬁeld. This leads to a preferential arrangement of dislocations into two-dimensional boundaries (subgrain boundaries), separating regions with slightly diﬀerent orientations (typically minutes of arc). There are other defects in crystals than these line (one-dimensional) defects. They can be classiﬁed according to their geometry as point, or zero-dimensional, defects (vacancies, interstitials); plane, or two-dimensional defects (twin boundaries, stacking faults), or three-dimensional (voids, precipitates). These defects also interact with dislocations, and consequently aﬀect the plastic deformation process, leading to hardening (e.g. precipitation hardening or work hardening) when dislocation displacements are hampered. Dislocations also play an important role in the mechanism of crystal growth.

290

Symmetry and Physical Properties of Crystals

T

–T

(b)

(a) b

T v u –T

T

b

(d) –T

(c)

b

T u

v

(f)

–T

(e)

Figure 13C.2: Schematic illustration of elastic and plastic deformation processes. (a) and (c) are identical and show an initial, strain-free state. (b) is the result of elastic deformation. (d) shows the plastic deformation stage in which an edge dislocation uv, which Burgers vector b, moves to the right in its glide plane. (e) shows the plastic deformation stage in which a screw dislocation, with the same Burgers vector b, moves toward the back of the ﬁgure. (f) is the plastically deformed state after the dislocation in (d) or (e) has moved across the sample. The density of dislocations in crystals is expressed as their total length per unit volume, hence as cm . cm−3 or cm−2 . It varies from zero in the perfect single crystals of silicon made for the production of microelectronic chips, to typically 1011 cm−2 in deformed metals.

Further reading D. Hull, D.J. Bacon, Introduction to Dislocations, 5th edn. (Elsevier, 2011) H. Föll, website on crystal defects (2001) http://www.tf.uni-kiel.de/matwis/amat/mw1 ge/index.html

Chapter 13 – Elasticity

291

References [1] D. Calecki, Physique des milieux continus, vol. 1, Mécanique et thermodynamique (Hermann, Paris, 2007) [2] A. Yeganeh-Haerl, D.J. Weidner, J.B. Parise, Science 257, 650–652 (1992)

Chapter 14

Elastic waves in crystals This chapter introduces an important application of the elasticity tensors: the propagation in crystals of acoustic waves, the velocity of which depends directly on the stiﬀness tensor. The end of this chapter discusses brieﬂy the relation between this macroscopic property and atom vibrations.

14.1. Introduction In the preceding chapter, we investigated the elastic behavior of crystalline solids submitted to static forces. These forces induce strains, which are connected to them through the elastic coeﬃcients. These coeﬃcients were ﬁrst measured using static approaches, which yield limited accuracy because the induced strains are very small. We will see in this chapter that, if the material is submitted to a strain wave, the velocity at which this wave propagates depends on the stiﬀness coeﬃcients of the material. These propagation velocities can be measured with an accuracy much higher than through static measurements. Therefore the stiﬀness coeﬃcients, from which the elastic coeﬃcients are deduced, are nowadays measured using techniques based on elastic wave propagation velocity. The elastic waves are excited in the crystal by transducers made from piezoelectric crystals (Sect. 15.3.6): when excited by a sinusoidal electric ﬁeld, they create a sinusoidal strain wave which is transmitted by contact to the crystal under investigation. In Sections 14.2, 14.3 and 14.4, the crystal is, as in all preceding chapters starting from Chapter 9, considered as a continuous medium. This assumption only holds as long as the wavelength of the elastic waves is much larger than the dimensions of the crystal’s unit cell. The frequency range used in applications is that of sound and ultrasound waves, gathered under the denomination of acoustic waves. Their frequency varies from 1 kHz to about 10 GHz, so that, considering the order of magnitude of the propagation velocity of sound in crystal materials (some 103 m s−1 ), the condition is satisﬁed. Nevertheless, it is worthwhile understanding the connection between this macroscopic approach and the microscopic treatment which directly takes into consideration

© Springer Science+Business Media Dordrecht 2014 C. Malgrange et al., Symmetry and Physical Properties of Crystals, DOI 10.1007/978-94-017-8993-6_14

293

294

Symmetry and Physical Properties of Crystals

the atomic arrangement and the binding forces between atoms. This is done in the last section, using a highly simpliﬁed model (a linear chain of equidistant identical atoms) which however provides insight into the behavior of a real crystal (three-dimensional unit cell, and several atoms per unit cell). These results are important, and they are given without derivation in Section 14.5.3.

14.2. Plane elastic waves Consider a solid submitted to an elastic perturbation, and a small volume element dv of this solid centered at a point with position vector r0 at rest. Its position at time t becomes: r(t) = r0 + u(r0 , t)

(14.1)

where u(r0 , t) is the displacement vector. The resultant F of the forces applied to this element dv is, using (11.3), such that:

∂Tij + fi dv Fi dv = ∂xj and, applying Newton’s second law:

∂Tij ∂ 2 xi + fi dv = (ρdv) 2 ∂xj ∂t

(14.2)

where ρ is the mass per unit volume of the solid. If the bulk forces f are zero or considered to be negligible, as we assume in the rest of this chapter, then: ∂ 2 xi ∂Tij =ρ 2 . (14.3) ∂xj ∂t Using (14.1),

and (14.3) becomes:

∂ 2 ui ∂ 2 xi = 2 ∂t ∂t2 ∂Tij ∂ 2 ui =ρ 2 . ∂xj ∂t

(14.4)

We can relate the components Tij to the partial derivatives of the components ui with respect to the position variables. The stress tensor Tij is related to the strain tensor Skl through the stiﬀness tensor cijkl (Eq. (13.1b)). Furthermore (Eq. (12.10)),

1 ∂uk ∂ul + . Skl = 2 ∂xl ∂xk We thus obtain: Tij = cijkl Sk

1 = cijkl 2

∂ul ∂uk + ∂xl ∂xk

Chapter 14 – Elastic waves in crystals and

∂Tij 1 = cijkl ∂xj 2

295

∂ 2 uk ∂ 2 ul + ∂xj ∂xl ∂xj ∂xk

.

The two terms on the right-hand side of this equation are equal since we sum over j, k and l. We can thus write:

2 ∂ ul ∂Tij = cijkl ∂xj ∂xj ∂xk and Equation (14.4) becomes:

cijkl

∂ 2 ul ∂xj ∂xk

=ρ

∂ 2 ui . ∂t2

(14.5)

We now show that the general solution to this equation has the form: s · r s · r + Be G t + . u(r, t) = AeF t − v v For simplicity, we restrict consideration to the ﬁrst term in this solution: s j xj s · r = AeF t − . u(r, t) = AeF t − v v This is the equation of a plane wave propagating along a direction parallel to unit vector s, with components si , because sj xj , hence the phase of the wave, is constant over any plane perpendicular to vector s (Fig. 14.1). If we consider any point M with coordinates xj , the plane P perpendicular to s and going through M intersects axis O, parallel to s, at H the projection of M and of all points of the plane onto O. For all points M in the plane, OM · s = xj sj = OH = and we can write:

s · r = AeF t − , (14.6) u(r, t) = AeF t − v v a plane wave whose wave planes move parallel to s, at velocity v. Unit vector e, whose components are noted ei , is called the polarization vector of the wave.

M r O s

H

P

Figure 14.1: Plane P perpendicular to unit vector s. This plane is the locus of points M for which s · r = s · OM = OH = const = .

296

Symmetry and Physical Properties of Crystals

Consider the form (14.6) of the displacement, and calculate its derivatives with respect to time and space, in order to substitute them into (14.5): ∂ 2 ui = Aei F , ∂t2 ∂ul sk = −Ael F ∂xk v

and

sj sk ∂ 2 ul = Ael 2 F ∂xj ∂xk v

where F and F are respectively the ﬁrst and second derivatives of F (w) with respect to w. Equation (14.5) becomes: cijkl el so that

sj sk F = ρei F v2

cijkl sj sk el = ρ v 2 ei .

(14.7)

Γil = cijkl sj sk

(14.8)

We set: and Equation (14.7) can be written as: Γil el = ρv 2 ei .

(14.9)

This equation shows that vector e is an eigenvector of matrix {Γil }, and that the eigenvalue associated to it is equal to ρv 2 . The terms in matrix {Γil } relate a vector to another vector. They are therefore the coeﬃcients of a rank-2 tensor [Γ] (Sect. 9.4.2), called the Christoﬀel tensor. This tensor is symmetric, since: Γli = cljki sj sk = ckilj sj sk because cαβ = cβα (Sect. 13.4). Also, since tensor cijkl is symmetric with respect to i and j and with respect to k and l (Sect. 13.2.2): Γli = cikjl sk sj

and

Γli = Γil .

Because matrix Γ is real and symmetric, it has three orthogonal eigenvectors. The eigenvalues are the solutions of the following equation, called the Christoffel equation: Γ11 − ρv 2 Γ12 Γ13 2 = 0. Γ12 Γ22 − ρv Γ23 2 Γ13 Γ23 Γ33 − ρv Once the eigenvalues are known, it is easy to deduce the eigenvectors, i.e. the polarization vectors of the corresponding elastic wave.

Chapter 14 – Elastic waves in crystals

297

Expanding the expression of one of the coeﬃcients Γil , for example Γ11 : Γ11 = c1111 s21 + c1121 s1 s2 + c1131 s1 s3 + c1211 s2 s1 + c1221 s22 + c1231 s2 s3 + c1311 s3 s1 + c1321 s3 s2 + c1331 s23 . Hence, using for the cijkl the two-subscript notation with α and β: Γ11 = c11 s21 + c66 s22 + c55 s23 + 2 (c16 s1 s2 + c15 s3 s1 + c56 s2 s3 ) . The other Γij coeﬃcients can be calculated in the same way, and the result is given in the form of Table 14.1. Each row of the table gives, for the coeﬃcient Γil indicated at the beginning of the row, the elastic coeﬃcients to be associated to each of the six terms s21 , s22 , s23 , s2 s3 , s3 s1 , s1 s2 in the sum. Table 14.1: Table showing the form of the components Γij of Christoffel’s tensor s21

s22

s23

s2 s3

s3 s1

s1 s2

Γ11

c11

c66

c55

2 c56

2 c15

2 c16

Γ22

c66

c22

c44

2 c24

2 c46

2 c26

Γ33

c55

c44

c33

2 c34

2 c35

2 c45

Γ23

c56

c24

c34

c44 +c23

c45 +c36

c46 +c25

Γ31

c15

c46

c35

c45 +c36

c13 +c55

c14 +c56

Γ12

c16

c26

c45

c25 +c46

c56 +c14

c12 +c66

In conclusion, three elastic waves can propagate in a crystal. The propagation velocity vj of each of these waves j, the phase velocity, is deduced from the corresponding eigenvalue ξj = ρ vj2 of the matrix {Γil } associated with the Christoﬀel tensor. The corresponding polarization vector ej is the eigenvector associated to ξj . The three polarization vectors are mutually orthogonal.

14.3. Application to a cubic crystal The stiﬀness matrix of a cubic crystal is expressed, in a system of axes parallel to the basis vectors of the crystal lattice: ⎛ ⎞ 0 0 c11 c12 c12 0 ⎜ c12 c11 c12 0 0 0 ⎟ ⎜ ⎟ ⎜ c12 c12 c11 0 0 0 ⎟ ⎟. c=⎜ ⎜ 0 0 ⎟ 0 0 c44 0 ⎜ ⎟ ⎝ 0 0 0 0 c44 0 ⎠ 0 0 0 0 0 c44

298

Symmetry and Physical Properties of Crystals

The Christoﬀel tensor coeﬃcients can then be expressed as: Γ12 = (c44 + c12 ) s1 s2 Γ11 = c11 s21 + c44 s22 + s23 2 2 2 Γ22 = c11 s2 + c44 s3 + s1 Γ23 = (c44 + c12 ) s2 s3 2 2 2 Γ31 = (c44 + c12 ) s3 s1 . Γ33 = c11 s3 + c44 s1 + s2 Their value depends on the propagation direction s of the plane wave. The next two sections deal with two special cases.

14.3.1. Propagation of a plane wave along direction [100] s1 = 1,

In this case:

s2 = s3 = 0.

The only non-zero coeﬃcients of the Christoﬀel tensor are thus: Γ11 = c11 ,

Γ22 = c44 ,

Γ33 = c44 .

The propagation velocities must satisfy equation: c11 − ρv 2 0 0 2 − ρv 0 0 c 44 0 0 c44 − ρv 2 the obvious solutions of which are: v1 =

= 0,

c11 ρ

with eigenvector (1, 0, 0) so that the wave is longitudinal (Fig. 14.2a), and c44 v2 = v3 = ρ for which the eigenvectors are vectors of the subspace formed by vectors (0, 1, 0) and (0, 0, 1), in other words all vectors perpendicular to vector s: the wave is transverse (Fig. 14.2b). x3

x3

O x1

e1

s

e2

O

x2

s

x2

x1

(a)

(b)

Figure 14.2: Polarization vectors for waves propagating in a cubic crystal along direction [100]: (a) longitudinal wave; (b) transverse wave

Chapter 14 – Elastic waves in crystals

299

14.3.2. Propagation along direction [110] 1 s1 = s2 = √ , 2

In this case:

s3 = 0.

The only non-zero values of Christoﬀel’s tensor are: Γ11 =

c11 + c44 , 2

Γ22 =

c11 + c44 , 2

Γ33 = c44 ,

Γ12 =

The propagation velocities must satisfy equation: c +c c44 + c12 11 44 − ρv 2 0 2 2 + c + c c c 44 12 11 44 0 − ρv 2 2 2 0 0 c44 − ρv 2

c44 + c12 . 2

= 0.

Vector (0, 0, 1)is an obvious eigenvector, and the associated propagation velocity is v3 = c44 /ρ (Fig. 14.3). This wave is transverse. The eigenvalues v1 and v2 are solutions of:

2

c11 + c44 c44 + c12 2 2 − ρv − =0 2 2

hence v1 =

2c44 + c12 + c11 2ρ

and

v2 =

c11 − c12 . 2ρ

It is easy to show that√the polarization vector of the wave with propagation velocity v1 is e1 = (1/ 2)(1, 1, 0), so that the wave is longitudinal because e1 is parallel to s. √ The polarization vector of the wave with propagation velocity v2 is e2 = (1/ 2)(1, −1, 0), so that this is a transverse wave. x3 e3 e2

O s

x1

e1

x2

Figure 14.3: Polarization vectors for a wave propagating in a cubic crystal along direction [110]: (e1 ) and the wave is longitudinal, (e2 , e3 ) and the waves are transverse Notes: 1.

We found longitudinal and transverse waves to be the solutions in the two above cases, but these are very special cases. For a general propagation direction, the vibration modes are neither purely longitudinal

300

Symmetry and Physical Properties of Crystals nor purely transverse. The wave whose polarization vector is closest to the propagation direction s (i.e. for which the angle between e and s is smallest) is called quasi-longitudinal and the two other waves are called quasi-transverse.

2.

The velocity v is a phase velocity. In the case of a sine wave

k u(r, t) = Ae cos(ωt − k · r) = Ae cos(ωt − ks · r) = Ae cos ω t − s · r , ω the phase velocity v is equal to ω/k. We found above that the value of v does not depend on the angular frequency ω. Thus the crystal material is non-dispersive for acoustic waves. However it is anisotropic, and this velocity depends on the direction of vector k since the Christoﬀel tensor [Γ] depends on it. The group velocity vg , with components (vg )i = ∂ω/∂ki , which is the propagation direction of energy, is generally no more parallel to the wave vector.

3.

We showed (Sect. 12.4) that the relative volume variation of a deformed solid is equal to the trace of the strain tensor: ∂ui = div u. ∂xi In the special case of a transverse wave, it is easy to show that div u = 0. If one of the axes, for example Ox1 , is chosen parallel to the propagation vector s, the only non-zero components of u are u2 and u3 and, since they do not depend on x2 and x3 , div u = 0 and propagation occurs with no change in volume. In contrast, propagation of any other waves, for which div u = 0, entails expansion and compression regions in the solid.

14.4. Isotropic solid case This case is easily deduced from the propagation in a cubic crystal, by considering a general direction and using relation (13.7b) which connects the stiﬀness coeﬃcients of an isotropic material: c44 =

c11 − c12 . 2

Consider for example propagation direction [100] in a cubic material. From the results of Section 14.3.1, one longitudinal wave, with propagation velocity v , and transverse waves, with propagation velocity vt , can propagate, with c11 c44 vt = . v = ρ ρ Using the Lamé coeﬃcients λ and μ (see Sect. 13.6.2) such that: λ + 2μ = c11

μ = c44 ,

Chapter 14 – Elastic waves in crystals

301

the velocities of the longitudinal and transverse waves, v and vt respectively, become: λ + 2μ μ v = and vt = . ρ ρ The ratio of these longitudinal and transverse wave velocities is: λ 2μ + λ v = 2+ . = vt μ μ This ratio is always larger than 1. Hence, in an isotropic material, the longitudinal elastic waves propagate faster than the transverse elastic waves. Of course the same results would be obtained using the results of Section 14.3.2, derived for a propagation direction parallel to [110].

14.5. Microscopic approach – Crystal lattice dynamics Till now, we considered the crystal to be a continuous and homogeneous medium. It is worthwhile understanding how this macroscopic approach can be connected to a microscopic description involving the vibrations of the atoms. At equilibrium, the average interatomic distance in a crystal is the one which minimizes the crystal’s energy. If an atom is moved away from its equilibrium position, it is submitted by its neighbors to restoring forces which cause it to oscillate around its equilibrium position. These oscillations are transmitted to the neighboring atoms, thus creating within the solid an elastic wave which propagates in the crystal. The full treatment of atomic vibrations in a crystal, crystal lattice dynamics, involves no major diﬃculty, but it implies a rather cumbersome algebraic approach, with a wealth of subscripts, which is beyond the scope of this book. Nevertheless, the main characteristics of the results can be deduced from the simple model of a one-dimensional crystal, i.e. a linear chain of atoms. We will start out by working out the case of a chain of identical atoms, then that of a chain containing two types of atoms. These two examples provide the essential results of the full treatment.

14.5.1. Linear chain of identical atoms Consider a linear chain of N identical atoms, with mass M , the same distance a apart (Fig. 14.4). The atom displacements in the chain are assumed to be small enough that a series expansion to ﬁrst order of the energy with respect to the displacement be valid, which is equivalent to considering a harmonic potential. Furthermore, we assume that the forces between atoms are restricted to forces between nearest neighbors. We can thus imagine a chain of atoms connected by springs with the same coeﬃcient K.

302

Symmetry and Physical Properties of Crystals A0

a

A1

Aj –1

Aj

Aj +1

AN – 2

AN –1 x

O

Figure 14.4: One-dimensional chain consisting of a single kind of atoms, with mass M, at the same distance a from one another The force between two atoms is a restoring force proportional to the diﬀerence in distance between the displaced and the undisplaced atoms. There are N atoms, denoted as A0 , A1 , . . ., Aj , . . ., AN −1 . Atom j is, at equilibrium, at position x0j = ja, and, if it is displaced by uj , it is submitted to two forces, with respective algebraic values (Fig. 14.5): (a) K(uj−1 − uj ), the force exerted by atom j − 1, (b) K(uj+1 − uj ), the force exerted by atom j + 1. Their resultant Fj is: Fj = K(uj+1 + uj−1 − 2uj ). A0 O

Aj –1

a

Aj

Aj +1 x

uj –1

uj

uj +1

Figure 14.5: Displacement of the atoms in the one-dimensional chain. The positions of the atoms at equilibrium are the empty circles and the positions after displacement are the full circles. Applying Newton’s second law to the j-th atom, we obtain the equation for its motion: ∂ 2 uj (14.10) M 2 = K(uj+1 + uj−1 − 2uj ) ∂t thus altogether N equations for the N atoms. This system of N equations simpliﬁes considerably if we seek a solution where all the atoms have a sinusoidal movement with the same amplitude, the displacement being in the form of a plane monochromatic wave. For atom j: uj = A cos(kx0j − ωt) = A cos(kja − ωt) = A [exp i(kja − ωt)]

(14.11)

where means “real part of”. We set vj = exp i(kja − ωt), and we seek vj as a solution of Equation (14.10), which becomes ∂ 2 vj (14.12) M 2 = K(vj+1 + vj−1 − 2vj ). ∂t

Chapter 14 – Elastic waves in crystals

303

Since this equation is linear, uj will be a solution if vj is. We obtain: ∂ 2 vj = −ω 2 vj , ∂t2 vj−1 = e−ika vj

and

vj+1 = eika vj .

Equation (14.12) becomes: K K [2 − (e−ika + eika )] = 2 (1 − cos ka) M M

K ka ω 2 = 4 sin2 M 2 ω2 =

and

ω (k) = 2

ka K sin . M 2

(14.13)

The ω(k) curve is called the dispersion curve. It is periodic, with period equal to 2π/a (Fig. 14.6). Furthermore it is symmetric. It is therefore suﬃcient to consider half a period, for example 0 < k < π/a. K 2 — M

–– a

0

– a

k

Figure 14.6: Dispersion curve ω(k) of a linear chain consisting of identical equidistant atoms with mass M We notice that the dispersion relation (14.13) does not depend on j. Thus the N equations (14.12) lead to a single dispersion relation, which justiﬁes the choice we made of a sinusoidal displacement wave (14.11). However, we started out from N coupled oscillator equations, which means that if a single atom starts vibrating, it will not continue vibrating with the same amplitude. It transfers energy to its neighbors in a complicated way. The sine-wave solutions we sought are collective oscillations, uncoupled (independent) from one another, called the normal modes. Each mode corresponds to one well-deﬁned value of k and one well-deﬁned value of ω; hence, in the language of quantum physics, it is a stationary state. The number of normal modes is equal to the

304

Symmetry and Physical Properties of Crystals

number of equations we started from, N . If we want each atom to have the same environment, we must assume that N is very large, and that the chain is closed on itself (Born and Von Karman’s periodic boundary conditions). This implies that atom j coincides with atom j + N , so that uj = uj+N , and eikN a = 1, so that: kN a = 2pπ with p an integer 2pπ . Na There are thus N values of k in one period 2π/a, for example between −π/a and π/a. and

k=

We now look at two limiting cases: k very small, i.e. k π/a and k = π/a. If k π/a, then λ a. The wavelength is very large compared to the interatomic distance, and we expect to retrieve the results obtained when we assume the medium to be continuous. We notice that, in this case, many atoms have almost identical motions, and thus the discrete character of the chain vanishes. Equation (14.13) becomes ω ≈ ka K/M and the phase velocity vϕ = ω/k is: ω K =a . k M It is independent of k. The crystal is non-dispersive for such waves, in agreement with the result of the macroscopic treatment, and the velocity of the acoustic waves va is: K va = a . (14.14) M If k = π/a, Equation (14.11) becomes uj = A cos (ωt − jπ). There is no propagation any more, and two neighboring atoms, j and j + 1, vibrate in phase opposition. The maximum angular frequency ωm of the associated waves is given by: K ωm = 2 M whence a cutoﬀ frequency fc = ωm /2π which can be related to the above acoustic wave velocity va determined in (14.14): va 1 K fc = = . (14.15) π M πa The results obtained with this extremely simple model can be generalized to the case of a real monoatomic crystal. It can be shown that there are three dispersion curves for one propagation direction of the wave. Each curve is

Chapter 14 – Elastic waves in crystals

305

associated to one of the polarization vectors determined at the beginning of this chapter, and its slope at origin is the associated propagation velocity. This one-dimensional model can be used to check that the frequency range of acoustic waves does correspond to the linear part of these dispersion curves. The order of magnitude of the cutoﬀ frequency deﬁned above (Eq. 14.15) can be calculated from the order of magnitude of the acoustic wave velocity va , some 103 m s−1 : we choose arbitrarily 3 × 103 m s−1 . If we assume an interatomic distance on the order of 2 Å, we obtain a cutoﬀ frequency on the order of 5 THz. The acoustic wave range does not extend beyond a few GHz, it is thus indeed in the linear part of the dispersion curve.

14.5.2. Linear chain with two diﬀerent atoms We now consider a linear chain of atoms, with period a, containing two types of equidistant atoms, with mass respectively M and m (Fig. 14.7). The coordinate x0j of the j-th atom at equilibrium is x0j = ja/2. a M

m

Figure 14.7: One-dimensional chain, with period a, consisting of two types of atoms, with mass M and m, a distance a/2 apart During motion, the coordinate xj of this atom becomes: xj = j(a/2) + uj . As in the case of the monoatomic chain, we model the interaction force between nearest neighbor atoms with a harmonic restoring force, the equivalent of a spring with stiﬀness K. The force on the j-th atom is then given by: Fj = K(uj+1 − uj ) + K(uj−1 − uj ). The equations of motion are respectively M

∂ 2 uj = K(uj+1 + uj−1 − 2uj ), ∂t2

(14.16a)

for atom j with mass M , and m

∂ 2 uj+1 = K( uj+2 + uj − 2uj+1 ) ∂t2

(14.16b)

for atom j + 1 with mass m. As in the preceding case, we look for a solution having the form of a sinusoidal wave: uj = A [ei(kja/2−ωt) ]

and

uj+1 = αA [ei(k(j+1)a/2−ωt) ]

306

Symmetry and Physical Properties of Crystals

where α is the ratio of the respective displacement amplitudes of masses m and M . We obtain: −M ω 2 = K[α(eika/2 + e−ika/2 ) − 2] −mαω 2 eika/2 = K[(eika + 1) − 2αeika/2 ] so that M ω 2 = 2K [1 − α cos ka/2]

(14.17a)

2

mαω = 2K [α − cos ka/2] .

(14.17b)

From Equations (14.17a) and (14.17b): α=

2K cos(ka/2) 2K − M ω 2 . = 2K cos(ka/2) 2K − mω 2

This implies 2

2

2

(2K − mω )(2K − M ω ) = 4K cos so that mM ω 4 − 2K(m + M )ω 2 + 4K 2 sin2

2

ka 2

ka 2

= 0.

This is a second-degree equation in ω 2 , with solutions: 1/2 K(m + M ) ± (m + M )2 K 2 − 4K 2 mM sin2 (ka/2) 2 ω = mM so that ω2 =

1/2 ! K . (m + M ) ± (m + M )2 − 4mM sin2 (ka/2) mM

The ω(k) curve has two branches (Fig. 14.8). Their limiting values for k π/a and for k = π/a can be easily calculated. If k π/a, sin ka/2 ≈ ka/2 1 and we obtain: (m + M ) K and ω ≈ ka . ω ≈ 2K mM 2(m + M ) The corresponding values of α are −M/m and 1. The ﬁrst solution corresponds to point A in Figure 14.8. The atoms with masses m and M respectively vibrate in phase opposition and their center of mass is at rest (Fig. 14.9a). If the chain consists of an alternation of positive and negative ions, their motion leads to an electric polarization of the material. This gives a possibility of interacting with electromagnetic waves which leads, in particular, to wave absorption in the relevant frequency range. These frequencies happen to be those of optical electromagnetic waves. This is why this branch of the dispersion curve is called the optical branch or the optical mode.

Chapter 14 – Elastic waves in crystals

307

K(m+M) 2 ——— A mM

–– a

K 2— m

B

K 2— M

C

– a

0

k

Figure 14.8: Dispersion curve ω(k) for a periodic linear chain consisting of two types of equidistant atoms, with masses respectively M and m

(a)

(b)

Figure 14.9: Vibration modes for a periodic linear chain consisting of two types of equidistant atoms, in the approximation k π/a, so that λ 2a. For clarity, (i) we assume the vibrations to be transverse, and not longitudinal, and (ii) the wavelength is not extremely large with respect to period a. (a) Optical branch: the atoms with masses m and M respectively vibrate in phase opposition and their center of mass is at rest. (b) Acoustic branch: the two types of atoms vibrate in phase with the same amplitude.

308

Symmetry and Physical Properties of Crystals

The second solution corresponds to long wavelength acoustic waves. Both types of atoms vibrate in phase with the same amplitude (Fig. 14.9b). The material is no more dispersive (ω/k is constant) and the propagation velocity v is equal to ω/k: v=a

K . 2(m + M )

This is the equivalent of the propagation velocity of sound waves. If k = π/a, sin ka/2 = 1 and the two solutions for ω 2 are: K K and ω= 2 . ω= 2 m M The corresponding values of α are α = ∞ and α = 0. This limit corresponds to a half-wavelength equal to a, the distance between atoms of the same type. In the ﬁrst solution, mass m oscillates and mass M is at rest (point B in Fig. 14.8). It is no surprise that the frequency then depends only on mass m. In the second case, mass M oscillates and mass m is at rest (point C on Fig. 14.8).

14.5.3. Extension to the real crystal case The simpliﬁed theory we just presented makes it possible to understand the results for a real three-dimensional crystal. The dispersion curves ω(k) are then represented for a given direction of vectors k. The results are as follows: The dispersion curves feature 3 acoustic modes, analogous to the single acoustic mode of the linear chain. The slopes at origin of these modes are equal to the propagation velocities of the acoustic waves determined under the macroscopic theory. If two velocities are the same in some propagation direction, there are only two acoustic modes, one of them being degenerate. If the crystal contains one single atom per primitive unit cell, there are only acoustic modes. If the crystal contains two atoms per unit cell, there are, additionally, three optical modes, the properties of which are similar to those of the optical mode of the linear chain. The optical modes can also be degenerate. If the crystal contains p atoms per unit cell, there are 3p modes, 3 of which are acoustic modes and 3(p − 1) are optical modes. In all cases, the linear parts of the acoustic modes, near the origin of the dispersion curves, are compatible with the assumptions of continuity and homogeneity of the material, and consistent with the macroscopic results on the propagation of acoustic waves.

Chapter 14 – Elastic waves in crystals

309

14.6. Exercises Exercise 14.1 Consider the propagation of elastic waves in a crystal with mass per unit volume ρ. 1.

The crystal is monoclinic, and c is the basis vector parallel to the 2-fold axis or perpendicular to the mirror. We consider an elastic wave with wave-vector parallel to direction [001]. (a) Write down Christoﬀel’s matrix. (b) Determine the velocity and the polarization of the waves which propagate in the crystal.

2.

Same questions for an orthorhombic crystal, and a propagation direction parallel to direction [001].

3.

Same questions for a crystal having an n-fold rotation axis, with n > 2, and propagation direction parallel to direction [001].

4.

The crystal is hexagonal. The propagation direction is a general direction in the plane perpendicular to c. Show that a wave with polarization parallel to c, therefore transverse, propagates.

Exercise 14.2 The components of the stiﬀness tensor of diamond are to be determined from the measurement of the propagation velocities of elastic waves. Diamond is cubic and its mass per unit volume is 3.51 g cm−3 . 1.

Calculate the propagation velocity of longitudinal waves along direction [100].

2.

Calculate the propagation velocities along direction [111].

3.

The propagation velocities were measured in a diamond crystal for both of the above wave-vector directions. The results are as follows: For k parallel to [100]: velocity of transverse waves: vt = 11,196 m s−1 . For k parallel to direction [111]: velocity of the longitudinal wave: vl = 14,490 m s−1 , velocity of the transverse waves: vt = 13,239 m s−1 . Determine the components of the stiﬀness tensor of diamond.

Exercise 14.3 Consider a tetragonal crystal with point group 422. Determine the propagation velocity of elastic waves with wave-vector parallel to direction [110] in this crystal.

Chapter 15

Crystal thermodynamics. Piezoelectricity The aim of this chapter is to introduce crossed eﬀects, in which quantities related to diﬀerent areas of physics (thermal, mechanical, electrical) are connected through thermodynamics. It then deals with an example which is important through its many diverse applications: piezoelectricity. The mechanical properties of crystals were studied in Chapters 11, 12 and 13. We brieﬂy recall below their electrical and thermal properties. Usually, these properties are studied independently of one another. For example, the application of stress leads to a deformation of the material, the magnitude of which depends on the value of its elastic coeﬃcients. In a similar way, an electric ﬁeld applied to a crystal induces an electrical induction which depends on the dielectric permittivity of the material. In both of these examples, the physical quantities involved are of the same nature, or, to put it another way, belong to the same domain or area (mechanical and electrical respectively), and the eﬀects involved are called principal eﬀects. This is no more the case when, applying a variation in temperature (thermal constraint), we measure a variation in polarization (an electrical quantity, the phenomenon of pyroelectricity) or a strain (a mechanical quantity, the phenomenon of thermal expansion). The response does not belong to the same area, and the eﬀects involved are called crossed eﬀects. Thus, the response of a crystal to a constraint may have several aspects and imply various physical properties. The aim of this chapter is to examine the various responses of crystals to a given constraint. To introduce these eﬀects and the connections between them, it is necessary to assume the crystal to be in an overall thermodynamic state deﬁned by one parameter in each of the thermal, mechanical and electrical domains. This will be done in the ﬁrst section, and will make it possible to introduce various crossed eﬀects. We will then study more speciﬁcally two special crossed eﬀects, viz. the properties of pyroelectricity (Sect. 15.2) and piezoelectricity (Sect. 15.3) featured by some crystals.

© Springer Science+Business Media Dordrecht 2014 C. Malgrange et al., Symmetry and Physical Properties of Crystals, DOI 10.1007/978-94-017-8993-6_15

311

312

Symmetry and Physical Properties of Crystals

15.1. Crystal thermodynamics 15.1.1. Conjugate variables Mechanical quantities We have seen that, under the eﬀect of a stress represented by a tensor [T ], a material undergoes a strain [S] such that [S] = [s][T ] Sij = sijkl Tkl

or

and, in contracted notation (Sect. 13.3): Sα = sαβ Tβ .

(15.1)

[s] is the tensor of elastic compliances, which connects the response [S] of the crystal to the constraint [T ]. In a similar way, the stress is related to the strain by the tensor of elastic stiﬀnesses [c] according to the relation [T ] = [c][S] or

Tij = cijkl Skl

and in contracted notation Tα = cαβ Sβ . During a change in the strain dSij , the work δW received by unit volume of the system1 is given by Equation (13.5), i.e. δW = Tij dSij

or

δW = Tα dSα .

(15.2)

Tensors [S] and [T ] are the conjugate quantities, or conjugate variables, in the mechanical domain. Electrical quantities When submitted to an electric ﬁeld E, a material polarizes, and its polarization P, the dipole moment per unit volume, is P = ε0 [χ]E, where [χ] is the electrical susceptibility tensor. The electrical induction D is such that D = ε0 E + P = ε0 ([E] + [χ])E = ε0 [ε]E

(15.3)

1. Here we assume, for simplicity’s sake, that the stress and the strain are homogeneous. If this were not the case, we would have to write δW = Tij dSij dv, where the integral is performed over unit volume.

Chapter 15 – Crystal thermodynamics. Piezoelectricity

313

which can also be written as Di = ε0 εij Ej .

(15.4)

ε0 is the permittivity of vacuum, the value of which, in the international system (SI) of units, is 10−9 /36π = 8.8 × 10−12 , and [ε] is the electrical permittivity tensor which connects the response D of the crystal to the electric ﬁeld E. Relation (15.4) can be inverted by introducing the impermeability tensor [η], the inverse of the relative electrical permittivity tensor [ε]: Ei = ηij

Dj . εo

During a variation in induction dD, the work received by unit volume of the system is (see e.g. [1])2 δW = Ei dDi = E · dD.

(15.5)

D and E are the conjugate quantities in the electrical domain. Relation (15.3) must be altered for some materials which additionally feature a polarization P0 , the spontaneous polarization, in the absence of an electrical ﬁeld. For these materials: D = P0 + ε0 [ε]E

(15.6)

so that, in zero ﬁeld, D = P0 . These materials are called pyroelectric because, as we will see, this intrinsic polarization varies with temperature. They can only belong to some crystal classes3 (Sect. 9.5.2). Thermal quantities If we apply a reversible change in temperature dΘ to unit volume of a material, it receives per unit volume a quantity of heat δQrev : δQrev = Cexp dΘ 2. The exact form given by Landau and Lifshitz in [1] is δW = Ei dDi dv, where the integral must be taken over the whole volume, including vacuum if the dielectric does not occupy all of the space between conductors. We therefore assume here that the material ﬁlls all the space between conductors, and that E and D are homogeneous in the material. This makes it possible to refer to the work per unit volume of the material. 3. We recall that a crystallographic class includes all crystals with a given point group.

314

Symmetry and Physical Properties of Crystals

where Cexp is the heat capacity per unit volume of the material under the conditions of the experiment (e.g. at constant volume or at constant pressure). The quantity of heat is not one of the variables deﬁning the state of a system, and δQ is not a total diﬀerential. We must consider the entropy of the system S, deﬁned by its variation dS during a reversible transformation where the temperature changes from Θ to Θ + dΘ: dS =

Cexp δQrev = dΘ. Θ Θ

(15.7)

Entropy S and temperature Θ are the conjugate variables of the thermal domain.

15.1.2. Independent variables Consider a system with unit volume, deﬁned by three quantities, each of them chosen in one of the above domains, viz. the thermal, electrical and mechanical domains. In the thermal domain, we can choose temperature Θ or entropy S, which are scalars. In the electrical domain, the electric ﬁeld E or induction D, which are vectors deﬁned by three components. And in the mechanical domain the strain tensor or the stress tensor, both symmetrical tensors with six independent components each. The state of the system is thus deﬁned in total by 10 independent variables. For clarity, we actually consider the tensor form of tensors [T ] and [S], with the two-subscript notation Tij and Sij for their coeﬃcients,4 and will thus consider 13 variables which are only quasi-independent since three of them are equal to three others (Tij = Tji and Sij = Sji for i = j). We will then revert to the contracted notation and to the 10 independent variables. When the system changes state, its internal energy per unit volume U changes by dU such that dU = ΘdS + δW where dS is the change in entropy and δW the reversible work, so that here δW = Ei dDi + Tkl dSkl and dU = ΘdS + Ei dDi + Tkl dSkl . If we are interested in the internal energy of the system, the usual choice of independent variables is the entropy S per unit volume, the three components of induction Di , and the 9 components of strain Skl . We call these variables, which appear in the diﬀerential of the various terms in dU , the thermodynamic coordinates of the system, and we denote them as xi , with index i ranging 4. This makes it possible to clearly deﬁne the transition from the two subscripts ij to the single subscript α for the new tensors which will be introduced (thermal expansion and piezoelectricity).

Chapter 15 – Crystal thermodynamics. Piezoelectricity

315

from 1 to 13. The variables Θ, Ei and Tkl are the variables conjugate to the variables xi chosen to deﬁne the system. We note Xi the quantity conjugate to the thermodynamic coordinate xi , and thus dU = Xi dxi

(15.8)

using Einstein’s convention. The conjugate quantities Xi are intensive quantities, whereas the thermodynamic coordinates are often inaccurately described as extensive quantities. The electrical induction D is in fact homogeneous to a polarization, i.e. to a dipole moment per unit volume, and the components of the strain tensor deﬁne the relative variations in length. Thus the components Di and Skl cannot be considered as extensive quantities. Nevertheless they are quasi-extensive quantities because they are the ones to be multiplied by the value of the volume when the latter is no more unity. In practice, it is often more convenient to choose as independent variables deﬁning the system the conjugate quantities Xi . We are then led to considering another thermodynamic function5 of the system, the free enthalpy or Gibbs potential G, such that G = U − ΘS − Ei Di − Tkl Skl and dG = −SdΘ − Di dEi − Skl dTkl .

(15.9)

We thus conclude that ∂G ∂G ∂G Di = − Skl = − . (15.10) S =− ∂Θ Ej ,Tmn ∂Ei Θ,(Ej ),Tmn ∂Tkl Θ,Ei ,(Tmn ) In these formulas, the indexed variables that are taken to be constant during diﬀerentiation are indicated in parentheses when all of them are constant except for the one with respect to which diﬀerentiation is performed. For example, D1 is the derivative of G with respect to E1 at constant (Ei ), Θ, Tkl , meaning that E2 , E3 , Θ and all Tkl ’s are held constant. Using the above notation, with the xi representing the thermodynamic coordinates (the variables involved in the diﬀerential element of the elementary variation in internal energy (15.8)), and Xi their respective conjugate quantities, chosen here as deﬁning the state of the system, the relations (15.9) and (15.10) respectively take on the condensed form dG = −xi dXi and

∂G xi = − . ∂Xi (Xj )

(15.11)

5. The use of various thermodynamic functions depending on the independent variables of a problem is particularly well discussed in [2].

316

Symmetry and Physical Properties of Crystals

We can make a Taylor expansion of the value of each coordinate xi as a function of its value xi (0) in the initial state. We denote as Xj (0) the values of the conjugate quantities in the initial state. We obtain ∂xi (Xj − Xj (0)) (15.12) xi − xi (0) = ∂Xj 0 j

if we restrict the Taylor expansion to its ﬁrst term. This is equivalent to considering that the ﬁrst derivatives ∂xi ∂Xj 0 are constant, or that the variations (Xj − Xj (0)) are small. This is an approximation, usually valid, which will be used in this and the following chapters. Only in the last chapter shall we show that some special eﬀets (such as electrooptical and piezo-optical eﬀects) require the inclusion of higher order terms. The same would apply for other eﬀects such as non-linear elasticity, but we will not deal with them in this book. Using Equations (15.11), relation (15.12) can be written as ∂2G (Xj − Xj (0)) xi − xi (0) = − ∂Xj ∂Xi 0 j

or xi − xi (0) = Mij (Xj − Xj (0))

(15.13)

using Einstein’s convention for subscript j (ranging from 1 to 13) and setting ∂ 2 G . (15.14) Mij = − ∂Xj ∂Xi 0 Since the order of the diﬀerentiations does not matter: Mji = Mij . We thus deﬁned a symmetrical matrix with 13 rows and 13 columns, called the physical property matrix M . Consider an initial reference state at Θ = Θ0 , without stress so that Tkl = 0, and in zero electric ﬁeld, so that Ei = 0, and a ﬁnal state where Θ = Θ0 + ΔΘ, Ei = 0, Tkl = 0. In the reference state, Ei is zero, hence, according to Equation (15.4), induction Di is also zero, except if the crystal is naturally polarized, which is the case for pyroelectric crystals (Eq. (15.6)). For the latter the reference state has a spontaneous polarization P0 at Θ0 . Since the stress tensor Tkl is zero in the reference state, so is the strain Skl . Thus, in the reference state, S = S0 , Di = 0 (except for pyroelectrics where D0 = P0 ) and Skl = 0. Thus the only thermodynamic quantity with non zero

Chapter 15 – Crystal thermodynamics. Piezoelectricity

317

value xi (0) is S0 . The 13 components of the vector xi − xi (0) are therefore S − S0 = ΔS, Dj and Smn . A slightly more detailed presentation of Equations (15.13), using Einstein’s convention (Sect. 9.3.1), is the following: ∂2G ∂2G ∂2G ΔΘ − − (15.15a) E Tkl , i ∂Θ2 ∂Ei ∂Θ ∂Tkl ∂Θ ∂2G ∂2G ∂2G ΔΘ − Ei − Tkl , (15.15b) Dj = − ∂Θ∂Ej ∂Ei ∂Ej ∂Tkl ∂Ej ∂2G ∂2G ∂2G ΔΘ − Ei − Tkl . (15.15c) Smn = − ∂Θ∂Tmn ∂Ei ∂Tmn ∂Tkl ∂Tmn The partial derivatives are calculated for the reference state, assuming the variables other than those with respect to which derivation is performed to be constant. ΔS = −

Equations (15.15) connect the components of a 13-component vector y (ΔS, Dj , Smn ) to the 13 components of another vector Y (ΔΘ, Ei , Tkl ) via the physical property matrix deﬁned above in (15.14), i.e. yi = Mij Yj .

(15.16)

15.1.3. Principal eﬀects vs crossed eﬀects Some coeﬃcients of the matrix Mij are known and represent the principal eﬀects. They are the “diagonal” terms in the broad sense, which we recall below. The variation in entropy ΔS at zero electric ﬁeld Ei and stress Tkl , as a function of the variation in temperature, is C ΔQ = ΔΘ ΔS = Θ Θ where C is the heat capacity per unit volume of the material (at zero electric ﬁeld and stress). Similarly, if an electric ﬁeld Ei is applied (at zero ΔΘ and Tkl ), the induction Dj is given by Dj = εji Ei , where εji is the relative electrical permittivity tensor. We note that εij = εji since εij = −

∂2G ∂Ei ∂Ej

and the order of the derivations is irrelevant. The tensor [ε] is symmetrical. Applying a stress Tkl (at zero ΔΘ and Ei ) gives rise to a strain Smn such that Smn = smnkl Tkl . We note that smnkl = sklmn since smnkl = −

∂2G . ∂Tkl ∂Tmn

318

Symmetry and Physical Properties of Crystals

We retrieve the symmetry of tensor [s] which we already derived in Section 13.4. The non-diagonal terms correspond to the crossed eﬀects, and are pairwise equal since matrix Mij is symmetrical. Thus the system (15.15) can be rewritten as: ΔS = (C/Θ)ΔΘ + pi Ei + αkl Tkl ,

(15.17a)

Dj = pj ΔΘ + εji Ei + djkl Tkl ,

(15.17b)

Smn = αmn ΔΘ + dimn Ei + smnkl Tkl .

(15.17c)

In these expressions, we set: ∂2G ∂2G =− , ∂Ei ∂Θ ∂Θ∂Ei ∂2G ∂2G αkl = − , =− ∂Tkl ∂Θ ∂Θ∂Tkl ∂2G ∂2G =− . djkl = − ∂Tkl ∂Ej ∂Ej ∂Tkl pi = −

(15.18a) (15.18b) (15.18c)

The coeﬃcients pj (called the pyroelectric coeﬃcients) in Equation (15.17b) describe the pyroelectric eﬀect, i.e. a variation in spontaneous polarization under the inﬂuence of a change in temperature at zero stress and electric ﬁeld. We recall, from the beginning of this section, that the reference state for D in pyroelectric crystals is the spontaneous polarization P0 at the reference temperature Θ0 . The quantity Dj in Equation (15.17b) is then the component ΔPj of the variation in spontaneous polarization ΔP under the inﬂuence of the variation in temperature, i.e. ΔPj = pj ΔΘ. The same coeﬃcients describe the electrocaloric eﬀect (Eq. (15.17a)), i.e. the production of heat under the inﬂuence of an electric ﬁeld in pyroelectric crystals. The coeﬃcients αmn (Eq. (15.17c)) describe thermal expansion (strain Smn under the inﬂuence of a variation in temperature ΔΘ, with Smn = αmn ΔΘ) and also the piezocaloric eﬀect (Eq. (15.17a)), i.e. the production of heat ΔQ = ΘΔS = Θαkl Tkl under the inﬂuence of a stress Tkl . The coeﬃcients djkl (Eq. (15.17b)) describe the direct piezoelectric eﬀect, i.e. the appearance of a polarization under the inﬂuence of a stress Dj = Pj = djkl Tkl or, for pyroelectric crystals, the appearance of an additional polarization ΔPj = djkl Tkl . They also describe (Eq. (15.17c)) the appearance of a strain under the inﬂuence of an electric ﬁeld, Smn = dimn Ei . This is called the inverse piezoelectric eﬀect.

15.1.4. Summary of the various eﬀects The above results are summarized in Table 15.1. The various eﬀects are represented on Figure 15.1 by a drawing borrowed from [3].

Chapter 15 – Crystal thermodynamics. Piezoelectricity

319

Table 15.1: Table describing the physical eﬀects related to the coeﬃcients of the physical property matrix. The principal eﬀects are shaded. Thermodynamic coeﬃcients ΔΘ ΔS

Dj

Smn

Ei

Tkl

Heat capacity C/Θ

Electrocaloric eﬀect pi

Piezocaloric eﬀect αkl

Pyroelectricity pj

Electrical permittivity εji

Direct piezoelectric eﬀect djkl

Thermal expansion αmn

Inverse piezoelectric eﬀect dimn

Elasticity smnkl

ric effect p Pyroelect

Heat capacity

Thermal ex

oe

eff ec t

rm

[ T]

S

s

ic lor

e eff

ec t eff

Th erm

oe

tic

las

lec

tic

e Th

s

pansion [ ]

[ ct

]

] y [s

[ S]

it ca [ d] tic zo ec t las e E i c eff P i r t lec zoe pie t c Dire

D Inve rse

Electromechanical effects

Ele

c tr oc

Pe rm

alo

ric

eff ec tp y pie [] zoe lec t ric e ffec t [d ]

itti

vit

E

Figure 15.1: Schematic representation of the principal and crossed eﬀects (adapted from [3], by permission of Oxford University Press)

320

Symmetry and Physical Properties of Crystals

Two equilateral triangles are drawn with the same center and the same orientation. The thermodynamic coordinates (the xi , which are the entropy, electrical induction and strain) are placed at the vertices of the internal triangle (i). Their conjugate quantities (the Xi , which are the temperature, the electric ﬁeld and the stress) are placed at the vertices of the external triangle (e). The arrangement is such that two conjugate quantities are located on the same median of the triangles. The arrows indicate the paths from one quantity to another. Those connecting a quantity and its conjugate (arrow from e to i) represent the principal eﬀects. For example, the arrow connecting Θ to S (thermal domain) corresponds to a change in entropy due to a variation in temperature, i.e. the heat required to obtain a variation in temperature, and the physical quantity associated to this eﬀect is the heat capacity. The temperature vertex Θ of the external triangle can be connected to quantities from another domain in the internal triangle, viz. the electrical induction or the strain, and the associated arrows (from e to i) correspond to crossed eﬀects (pyroelectric eﬀect and thermal expansion). The straight line segments parallel to the sides of the triangle are paths from i to i or e to e. The area between two such parallel segments, such as the segment connecting Θ to E and the one connecting S to D, represent various eﬀects that couple two domains, here the thermal and the electrical domain; the various eﬀects are designated as thermoelectric.

15.1.5. Condensed representation of the physical property matrix The way we deﬁned it, the physical property matrix connects two 13-component vectors. We know that, because tensors Sij and Tij are symmetric, we can replace the nine components Sij and Tij by the 6 independent components Sα and Tα deﬁned in (13.3) and (13.4) respectively. Thus vectors yi and Yi become 10-component vectors and matrix M a 10 by 10 matrix (Fig. 15.2). The “diagonal” terms which connect the Sα and Tα are then the contracted elastic coeﬃcients sαβ . The crossed terms implying the Sα and Tα are the components diα and αβ which are deduced from components dijk and αij . We will show in Section 15.3.2 how to go over from the dijk to the diα . Let us see how we go over from the components αij of the thermal expansion tensor (equal to the piezocaloric tensor) to the contracted components αβ . If we apply a temperature variation ΔΘ at zero or constant electric ﬁeld and stress, the components of the strain tensor Smn can be written as: Smn = αmn ΔΘ, which we want to write as Sβ = αβ ΔΘ. It is clear that, for S11 , S22 and S33 , which are respectively equal to S1 , S2 and S3 , we simply set αβ = αmm . The same does not apply for β = 4, 5 or 6. For example, for β = 4, S4 = S23 + S32 = (α23 + α32 )ΔΘ = α4 ΔΘ if we set α4 = α23 + α32 .

Chapter 15 – Crystal thermodynamics. Piezoelectricity ⎛ ⎜ ⎜ ⎜ ⎜ ⎜ ⎜ ⎜ ⎜ ⎜ ⎜ ⎜ ⎜ ⎜ ⎜ ⎜ ⎝

ΔS D1 D2 D3 S1 S2 S3 S4 S5 S6

⎞

⎛

⎟ ⎜ ⎟ ⎜ ⎟ ⎜ ⎟ ⎜ ⎟ ⎜ ⎟ ⎜ ⎟ ⎜ ⎟ ⎜ ⎟=⎜ ⎟ ⎜ ⎟ ⎜ ⎟ ⎜ ⎟ ⎜ ⎟ ⎜ ⎟ ⎜ ⎠ ⎝

C T p1

p2 p3 α1 α2 α3 α4 α5 α6

p1 ε11 ε12 ε13 d11 d12 d13 d14 d15 d16

p2 ε12 ε22 ε23 d21

p3 ε13 ε23 ε33 d31

α1 d11 d21 d31 s11 s12 s13 s14 s15 s16

α2 d12 d22 d32 s12 s22

α3 d13 d23 d33 s13 s23 s33

α4 d14 d24 d34 s14 s24 s34 s44

321

α5 d15 d25 d35 s15 s25 s35 s45 s55

α6 d16 d26 d36 s16 s26 s36 s46 s56 s66

⎞⎛ ⎟⎜ ⎟⎜ ⎟⎜ ⎟⎜ ⎟⎜ ⎟⎜ ⎟⎜ ⎟⎜ ⎟⎜ ⎟⎜ ⎟⎜ ⎟⎜ ⎟⎜ ⎟⎜ ⎟⎜ ⎠⎝

ΔT E1 E2 E3 T1 T2 T3 T4 T5 T6

⎞ ⎟ ⎟ ⎟ ⎟ ⎟ ⎟ ⎟ ⎟ ⎟ ⎟ ⎟ ⎟ ⎟ ⎟ ⎟ ⎠

Figure 15.2: Physical property matrix Thus we conclude that for β = 1, 2, 3:

αβ = αmm ,

for β = 4, 5, 6:

αβ = αmn + αnm .

It is easy to check that this result remains valid for the piezocaloric eﬀect, which can be written as ΔS = αβ Tβ . In the following sections, we study more speciﬁcally two of the crossed eﬀects we just introduced, viz. pyroelectricity and piezoelectricity.

15.2. Pyroelectricity. Pyroelectric crystals Pyroelectric crystals feature a spontaneous polarization in the absence of an electric ﬁeld. They are crystals for which the centers of gravity of the positive and of the negative charges in the unit cell do not coincide. For these materials: D = P0 + ε0 [ε]E. In the absence of an applied electric ﬁeld, and at a given reference temperature Θ0 : D = P0 . This polarization is diﬃcult to evidence because the surface charges due to polarization are rapidly neutralized by free charges from the air or through conduction in the crystal. However, its variation as a function of temperature can be measured more easily, and this change (at zero electric ﬁeld and stress) ΔP = P(Θ)−P(Θ0 ) is related, according to Equation (15.17b), to the variation in temperature ΔΘ = Θ − Θ0 by ΔPi = pi ΔΘ

or

ΔP = pΔΘ.

p is a vector whose components are the pyroelectric coeﬃcients.

322

Symmetry and Physical Properties of Crystals

We showed (Sect. 9.5.2) that pyroelectricity can occur only in crystals belonging to one of the following point groups: 1, 2, 3, 4, 6, m, mm2, 3m, 4mm and 6mm. The best known pyroelectric crystal is tourmaline, whose variation in polarization with temperature was evidenced in antiquity. The materials most used in applications (especially for infrared radiation detectors) are ferroelectric materials because their pyroelectric coeﬃcients are usually higher. Ferroelectric crystals are pyroelectric crystals whose spontaneous polarization can be reversed under the inﬂuence of high enough an electric ﬁeld. These crystals generally undergo a phase change at a given temperature, called the Curie temperature Θc , above which they are no more pyroelectric. Therefore the pyroelectric coeﬃcients are usually negative in a representation where the components of the spontaneous polarization are positive, since the spontaneous polarization decreases with increasing temperature and ﬁnally disappears beyond Θc . Among the best known materials are potassium dihydrogen phosphate KH2 PO4 , usually denoted as KDP, and barium titanate BaTiO3 . The point group of KDP is mm2 (orthorhombic system) in the ferroelectric phase and ¯42m (tetragonal system) above its Curie temperature Θc equal to −150◦ C. Barium titanate has the perovskite structure (Sect. 8.2.4), with point group m¯3m (cubic system) above the Curie temperature Θc = 120◦ C. As temperature is reduced below Θc , its point group is 4mm (tetragonal system). It then undergoes more transitions, its point group becoming mm2 (orthorhombic system) at Θ = 5◦ C, then 3m (rhombohedral system) at Θ = −90◦ C. It remains ferroelectric in these three phases. Ferroelectric materials are often used in the form of ceramics, i.e. as powders submitted to compacting and sintering at high temperatures, because they are easier to manufacture than single crystals and they can be given any shape. Without special treatments, the microcrystals forming the ceramics have random relative misorientation and their polarization can take on all possible orientations. Their average polarization is then zero. To obtain a sizable polarization, the ceramic is submitted to a strong electric ﬁeld which orients the polarization of each of the domains in the grains in the direction closest to the electric ﬁeld consistent with the crystal symmetry and the grain orientation.

15.3. Piezoelectric crystals 15.3.1. Direct eﬀect and inverse eﬀect A piezoelectric crystal polarizes under the action of an applied stress (direct eﬀect) and, conversely, deforms when an electric ﬁeld is applied (inverse eﬀect). The direct eﬀect was discovered by Pierre and Jacques Curie in 1880. The inverse eﬀect was predicted the following year by Gabriel Lippman on the basis of thermodynamic considerations, and its existence immediately veriﬁed by the Curie brothers.

Chapter 15 – Crystal thermodynamics. Piezoelectricity

323

The direct piezoelectric eﬀect connects the polarization induced in the crystal P and the applied stress [T ]. This eﬀect shows up at zero electric ﬁeld, and we can write, in agreement with Equation (15.17b): Di = Pi = dijk Tjk .

(15.19)

The inverse piezoelectric eﬀect connects the quantities conjugate to [T ] and D, viz. the strain [S] and the electric ﬁeld E respectively. Equation (15.17c) shows that (15.20) Sij = dkij Ek . It is worth noticing the diﬀerence in the order of the subscripts in the piezoelectric coeﬃcients dijk for the direct and inverse eﬀects in Equations (15.19) and (15.20). This is due to the deﬁnition, in (15.18), of the coeﬃcients dijk : the ﬁrst subscript points to a diﬀerentiation of free enthalpy with respect to a component of E, while the two last ones point to diﬀerentiation with respect to a component of [T ]. The above conditions, viz. zero electric ﬁeld to describe the direct eﬀect, and zero stress to describe the inverse eﬀect, are fulﬁlled only in special geometries or for high sample symmetry. Usually, the electric and mechanical quantities are coupled, and we must consider, at constant temperature, the two coupled equations resulting from (15.17b) and (15.17c): Pj = εji Ei + djkl Tkl , Smn = dimn Ei + smnkl Tkl .

(15.21a) (15.21b)

15.3.2. Piezoelectric tensor [d] and its two-subscript notation Equation (15.19) shows that the coeﬃcients dijk connect the second-rank tensor [T ] with the vector P, a ﬁrst-rank tensor. They are therefore the coeﬃcients of a third-rank tensor (Sect. 9.4.2). The same conclusions are reached by considering Equation (15.20), where the coeﬃcients dkij connect the ﬁrst-rank tensor E to the second-rank tensor [S]. A third-rank tensor comprises 33 = 27 coeﬃcients. This number can here be reduced by taking into account the symmetry of the stress tensor, allowing the 9 coeﬃcients Tij to be replaced by the six coeﬃcients Tα (Eq. (13.3)). Suppose we apply a stress for which only the components T23 = T32 are nonzero. The resulting polarization is Pi = di23 T23 + di32 T32 = (di23 + di32 )T23 . Since we cannot distinguish di23 and di32 , we set: dijk = dikj which reduces the number of independent components of tensor [d] to 18. Using the contracted notation, we immediately see that Equation (15.19) can be written as: (15.22) Pi = diα Tα

324

Symmetry and Physical Properties of Crystals

provided we set diα = dijk

for α = 1, 2 and 3 (j = k),

(15.23a)

diα = 2dijk

for α = 4, 5, 6 (j = k).

(15.23b)

Now relation (15.22) can be written in matrix form. The components Pi form a column vector with three rows, the components Tα a column vector with six rows, and the table of coeﬃcients diα a matrix with 3 rows and 6 columns. We thus obtain ⎛ ⎞ T1 ⎛ ⎞ ⎛ ⎞ ⎜ T2 ⎟ ⎜ ⎟ d11 d12 d13 d14 d15 d16 P1 ⎜ ⎟ ⎝ P2 ⎠ = ⎝ d21 d22 d23 d24 d25 d26 ⎠ ⎜ T3 ⎟ . ⎜ T4 ⎟ ⎜ ⎟ P3 d31 d32 d33 d34 d35 d36 ⎝ T5 ⎠ T6 The inverse piezoelectric eﬀect can be written as: Sij = dkij Ek . We see that, using the deﬁnitions (15.23) of the coeﬃcients diα , and the contracted notation for tensor [S] (Eq. (13.4)), we can write: Sα = diα Ei . This relation becomes a matrix relation provided we use the matrix dT , transposed from the preceding one, i.e. dTαi = diα ⎛

or

⎜ ⎜ ⎜ ⎜ ⎜ ⎜ ⎝

S1 S2 S3 S4 S5 S6

⎞

⎛

⎟ ⎜ ⎟ ⎜ ⎟ ⎜ ⎟=⎜ ⎟ ⎜ ⎟ ⎜ ⎠ ⎝

and d11 d12 d13 d14 d15 d16

d21 d22 d23 d24 d25 d26

Sα = dTαi Ei d31 d32 d33 d34 d35 d36

⎞ ⎟⎛ ⎞ ⎟ E1 ⎟ ⎟ ⎝ E2 ⎠. ⎟ ⎟ E3 ⎠

15.3.3. Eﬀect of crystal symmetry on the form of the tensor The piezoelectric tensor, a material tensor, must be invariant under all the point symmetry operations of the crystal (Sect. 9.5.2). We remember that, in applying this principle, we must revert to the three-subscript notation of the piezoelectric tensor.

Chapter 15 – Crystal thermodynamics. Piezoelectricity

325

Centrosymmetric crystal A centrosymmetric crystal cannot be piezoelectric, since odd-rank tensors are identically zero for all crystals featuring a center of symmetry (Sect. 9.6.3). We can retrieve this result directly from Curie’s principle. The symmetry of the eﬀect (electrical polarization, with symmetry ∞m) must include the symmetry of the cause (crystal + stress). Stress is centrosymmetric. If the crystal also is centrosymmetric, the intersection of the symmetry groups of the stress and of the crystal features a center of symmetry, and this is incompatible with symmetry group ∞m. Examples of reduction in the number of non-zero coeﬃcients We can apply the direct inspection method (Sect. 9.6.2) to all crystallographic groups except for those which contain a 3-fold or 6-fold axis. For the latter, we must revert to the matrix method (Sect. 9.6.1). We give below a few examples of the use of the direct inspection method, while the result for all crystal groups is given in Table 15.2. 1.

Crystals with group 2 We choose axis Ox3 parallel to the 2-fold axis. Rotating the coordinate system by angle π around Ox3 changes the components xi of a vector into components xi such that x1 = −x1 ,

x2 = −x2 ,

x3 = x3 .

Coeﬃcients dijk transform as the product of 3 components, so that for example d111 = −d111 , and on the other hand they must be invariant in the coordinate system rotation, so that d111 = d111 , which means that d111 = 0. We understand from this example that, if the subscripts i, j and k include an even number (0 or 2) of the value 3, which implies an odd number of the set of 1’s and 2’s, dijk = 0. Reverting to the 2-subscript notation, we obtain the table ⎞ ⎛ 0 0 0 d14 d15 0 ⎝ 0 (15.24) 0 0 d24 d25 0 ⎠ . d31 d32 d33 0 0 d36 2.

Crystals with group m Let us choose Ox3 perpendicular to the mirror. The action of the mirror perpendicular to Ox3 on the coordinate system changes the components xi of a vector into components xi such that x1 = x1 ,

x2 = x2 ,

x3 = −x3 .

326

Symmetry and Physical Properties of Crystals This time the coeﬃcients dijk that contain an odd number of indices equal to 3 are zero. The tensor now has the form: ⎞ ⎛ 0 d16 d11 d12 d13 0 ⎝ d21 d22 d23 0 0 d26 ⎠ . 0 0 0 d34 d35 0 Adding a 2-fold axis perpendicular to this mirror, we check that, for the centrosymmetric group 2/m, all coeﬃcients are zero.

3.

Crystals with group 222 We again consider matrix (15.24), and now add the eﬀect of the existence of another 2-fold axis. Choosing axis Ox2 along this second 2-fold axis, the zero coeﬃcients are those containing an even number of 2’s. The tensor thus becomes: ⎞ ⎛ 0 0 0 0 d14 0 ⎝ 0 0 0 0 d25 0 ⎠ . 0 0 0 0 0 d36 The eﬀect of a third 2-fold axis would bring nothing more, since the existence of this third axis is the direct consequence of the existence of the two others. Equivalently, we can say that the generating elements of the group 222 are restricted to rotations by π around two perpendicular axes.

4.

We note that group 423, although it is not centrosymmetric, has a piezoelectric tensor that is identically zero (Exercise 15.1).

Note: a crystal belonging to a piezoelectric group does not necessarily feature a piezoelectric eﬀect. The values of the components of the piezoelectric tensor depend very much on the crystal itself, and in some cases the coeﬃcients are all zero even when measured with high sensitivity. In this respect, the piezoelectric tensor is diﬀerent from the elastic or thermal expansion tensors. Conversely, experimentally detecting a piezoelectric signal indicates beyond doubt the absence of centrosymmetry in a crystal. When possible, the piezoelectric test is therefore a valuable complement to structural diﬀraction data, for which the conclusion on the presence or absence of centrosymmetry is diﬃcult. Form of the piezoelectric tensors for all crystal groups Table 15.2 shows the non-zero coeﬃcients of the piezoelectric tensor for all crystal groups, and Table 15.3 gives some numerical values for the coeﬃcients diα , in units of 10−12 C N−1 .

Chapter 15 – Crystal thermodynamics. Piezoelectricity

327

Table 15.2: Form of the matrix representing the piezoelectric tensor for the various crystal groups Triclinic 1 Monoclinic

2 Ox 2

0 0 0

0 0

0 0 0 m Ox 2 0 0 0

222 Tetragonal 4

0

0 0

0 0 0 0 0 0 0 0 0 0 0 0 0

0 0 0 0 0 0

– 4

0 0 0 0 0 0 0 0 0 0 0

4mm

0 0 0 0 0 0 0 0 0 0 0 0 0

32 2 Ox 1

0 0 0 0 0 0 0 0 0 0 0 0 0

0 0 0 0 0

0 0 0 0 0

6

622

0 0 0 0 0 0 0 0 0 0

0 0 0 3m 0 0 0 0 m Ox 2 0 0 0

0 0 0 0 0 0

6mm

0 0 0 0 0 0 0 0 0 0 0 0 0

– 6

0 0 0 0 0 0 0 0 0 0 0 0

0 0 0 0 0

0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0

0 0 0 0 0 – 62m 0 0 0 0 m Ox 1 0 0 0 0 0 0

0 0 0 0 – 62m 0 0 0 0 0 m Ox 2 0 0 0 0 0 0

0 0 0 0 0 0 0 0 23 0 0 0 0 0 0 0 0 – 43m 0 0 0 0 0 0 0 0 Equal components Components with equal absolute values Component equal to minus twice the component shown as a full black circle to which it is connected

Cubic

432

0

mm2

0 0 0 0 0 0 0 0 0 0 0 0 0 0 0

Hexagonal

0 0 0

0 0 0 0 0 0 0 0 0 0 0 0 0 0 0

– 42m 2 Ox 1

3m m Ox 1

0 0 0 0

m Ox 3

0

0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0

3

0 0

0 0 0 0 0 0 0 0

422

Rhombohedral

2 Ox 3

0

0 Orthorhombic

0

0 0 0 0 0 0 0 0 0 but opposite signs

328

Symmetry and Physical Properties of Crystals Table 15.3: Numerical values of the piezoelectric coeﬃcients for some materials, in units 10−12 C N−1 (from [4]) KDP (¯42m)

d14

d36

1.4

23.2

d15

d22

d31

d33

74

20.77

0.86

16.23

SiO2 (32)

d11

d14

Quartz

– 2.3

– 0.67

GaAs (¯43m)

d14

LiNbO3 (3m)

– 2.7 (25◦ C) 2.63 (196◦ C) InSb (¯43m)

d14 – 2.35 (25◦ C)

15.3.4. Longitudinal piezoelectricity surface The longitudinal piezoelectricity surface is obtained by plotting, on any direction with unit vector s, a length equal to the modulus of d111 in the orthonormal set of axes (Ox1 x2 x3 ), where Ox1 is parallel to s. To represent this threedimensional surface, we perform sections by planes going through the origin. The sign of d111 is then indicated as we will see with the example below. Assume the components of the piezoelectric tensor are known in the orthonormal axis system (Ox1 x2 x3 ) associated to the crystal axes, and denoted in this set of axes as dijk . We obtain d111 from the dijk ’s through the usual rule (Sect. 9.4.1): d111 = a1i a1j a1k dijk where {aij } is the transformation matrix for going over from the set of axes (Ox1 x2 x3 ) to the set (Ox1 x2 x3 ). aij is the component parallel to axis Oxj of the unit vector parallel to Ox1 , here denoted as s. Calling si the components of s in the axis system (Ox1 x2 x3 ), we then have d111 = si sj sk dijk .

(15.25)

We can interpret Equation (15.25) as follows. Assume the experimental conditions are such that, when applying a uniaxial stress at constant temperature to a piezoelectric crystal, the electric ﬁeld in the crystal is zero (Fig. 15.3). According to (15.19), we would obtain a polarization Pi = dijk Tjk . In a set of axes (Ox1 x2 x3 ) such that axis Ox1 is parallel to the uniaxial stress, the latter

Chapter 15 – Crystal thermodynamics. Piezoelectricity

329

x3 T

x’1

s

x2

x1

Figure 15.3: Schematic illustration of the meaning of longitudinal piezoelectricity, a measure of the polarization normal to the faces of a crystal to which a uniaxial stress is applied , and we obtain P = d T . We see that d has only one component, T11 111 i i11 11 is the component of polarization parallel to the uniaxial stress. Thus, under these special experimental conditions, d111 is the component of polarization normal to the face of the crystal to which a uniaxial stress is applied.

Application to a crystal with point group 4mm: The non-zero components of the piezoelectric tensor are given in Table 15.2 and Equation (15.25) becomes d111 = s3 [(s21 + s22 )(d15 + d31 ) + s23 d33 ]. If we use the spherical coordinates of s (r = 1, θ, ϕ), we obtain d111 = cos θ[sin2 θ(d15 + d31 ) + cos2 θd33 ]. This longitudinal piezoelectricity coeﬃcient does not depend on azimuth ϕ. The longitudinal piezoelectricity surface is therefore a surface of revolution around the axis Ox3 , the 4-fold axis. Its section by a meridian plane is shown on Figure 15.4 for the case of barium titanate BaTiO3 in its tetragonal phase (between 120◦ C and 5◦ C). We note that for θ > π/2 the value of d111 is negative. This is why the sign − is inserted in the center of the lobe corresponding to the half-space with negative x3 .

15.3.5. Other forms of piezoelectric coeﬃcients The above piezoelectric coeﬃcients connect polarization to stress and relation (15.17b) shows that they are isothermal coeﬃcients (at constant temperature). For some applications, it is more convenient to express polarization as a function of strain, be it through isothermal or adiabatic (constant entropy) coeﬃcients. Let us focus on isothermal coeﬃcients. The thermodynamic variables must then be temperature, electric ﬁeld and strain. The thermodynamic function to consider is another Gibbs function G2 : G2 = U − ΘS − Ei Di , dG2 = −SdΘ − Di dEi + Tij dSij .

(15.26)

330

Symmetry and Physical Properties of Crystals 10–12 C/N 150 100 50

+

0 – 50

–

– 100 – 150

Figure 15.4: Intersection of the longitudinal piezoelectricity surface of a crystal of barium titanate (BaTiO3 ), with point group 4mm, by a plane passing through the 4-fold axis, which is an axis of revolution for this surface With the same approach as in Section 15.1.2 and Section 15.1.3, we obtain ΔS = (C/Θ)ΔΘ + pi Ei + λkl Skl ,

(15.27a)

Dj = pj ΔΘ + εji Ei + ejkl Skl ,

(15.27b)

Tmn = −λmn ΔΘ − eimn Ei + cmnkl Skl .

(15.27c)

Clearly the coeﬃcients pi are pyroelectric coeﬃcients at constant temperature and strain, while in Equations (15.17) they were the constant temperature and zero stress coeﬃcients. Their diﬀerence will be calculated in Section 15.4. We note that the coeﬃcients eijk appear with opposite signs. The explanation is simple, since they are obtained through: Dj = −

∂Dj ∂ 2 G2 ∂G2 from (15.26) and =− . ∂Ej ∂Skl ∂Ej ∂Skl

We set: ejkl = −

∂ 2 G2 . ∂Ej ∂Skl

On the other hand Tmn =

∂G2 ∂Smn

and

∂Tmn ∂ 2 G2 = = −eimn ∂Ei ∂Ei ∂Smnl

from deﬁnition (15.28). The opposite signs for the λij have the same origin.

(15.28)

Chapter 15 – Crystal thermodynamics. Piezoelectricity

331

In piezoelectricity problems involving constant temperature, we then use the two equations: Dj = εji Ei + ejkl Skl , Tmn = −eimn Ei + cmnkl Skl .

15.3.6. Applications Materials used Piezoelectric materials can be used under various forms: single crystal form: the best known is quartz, a natural crystal which is also manufactured, often as large single crystals with excellent quality (Fig. 1.3). Other important single crystal materials are berlinite (AlPO4 ), gallium orthophosphate (GaPO4 ), gallium arseniate (GaAsO4 ), lithium niobate (LiNbO3 ), lithium tantalate (LiTaO3 ). ceramics: if the piezoelectric material is also ferroelectric, it can be used in the form of a polarized ceramic, i.e. of a compacted and sintered powder, the grains of which are reoriented by applying a strong electric ﬁeld (see Sect. 15.2). Among the materials used in ceramic form are barium titanate (BaTiO3 ), potassium niobate (KNbO3 ), lead zirconate–titanate Pb(Zrx Ti1−x )O3 , designated as PZT. thin crystal ﬁlms polymers: some polymers such as polyvinylidene ﬂuoride (PVDF) become piezoelectric if their molecules are oriented by a mechanical or electrical process. Application areas There are many areas of application, and the list below is not exhaustive. Converting an electrical wave into an acoustical wave, i.e. production of ultrasound, and conversely conversion of an acoustic wave into an electrical signal for ultrasound reception. These two eﬀects make it possible to emit ultrasound waves and to receive those scattered by the medium. This is why they are used in medicine for echography and in sonars (the acronym for SOund Navigation And Ranging) to detect objects in water and determine their distance.6 In the range of audible frequencies, production of microphones and loudspeakers, in particular for cellular telephones. Pressure sensors: pressure on the piezoelectric material generates a measurable electrical signal. 6. The sonar was invented by Paul Langevin and Constantin Chilowski in 1917 and used during World War I.

332

Symmetry and Physical Properties of Crystals Micro-manipulators: an applied voltage generates a strain which leads to micro-displacements. Piezoelectric resonators: elastic waves propagate in a crystal as modes which depend on its shape, dimensions and nature. The piezoelectric effect, which couples the mechanical and electric quantities, makes it possible to generate these vibration modes. This produces resonators which vibrate, when an electrical signal is applied, at a perfectly deﬁned frequency, stable over long periods of time. Quartz watches thus use the resonance of a quartz tuning-fork shaped crystal to generate regular time pulses. The use of quartz crystals with special orientation, shape and dimensions make it possible to obtain resonators whose frequency practically does not vary with temperature. The resonance frequency of this type of oscillators is extremely sensitive to the mass of the crystal, yielding quartz balances capable of detecting extra masses on the order of an atomic monolayer. High voltage generation through application of a stress: this eﬀect is used in gas lighters.

15.4. Principal and crossed eﬀects under various conditions In the preceding sections (except for Sect. 15.3.5), the various tensors representing principal or crossed eﬀects connect a conjugate-type quantity to a thermodynamic coordinate-type quantity for constant values of the two conjugate quantities which do not enter the relation. For example tensor smnkl connects stress Tkl to strain Smn at constant temperature and zero or constant electric ﬁeld. Equation (15.17c) then yields: Smn = smnkl |E,Θ Tkl . and smnkl |E,Θ is the isothermal elastic coeﬃcient. The same coeﬃcient at constant entropy, ΔS = 0 and zero electric ﬁeld is denoted as smnkl |E,S and we now determine the relation connecting them. If ΔS = 0, the change in temperature is no more zero. It is given by Equation (15.17a), i.e. 0 = (C/Θ)ΔΘ + αkl Tkl

and

ΔΘ = −(Θ/C)αkl Tkl .

Equation (15.17c) becomes Smn = −αmn (Θ/C)αkl Tkl + smnkl Tkl = (−αmn (Θ/C)αkl + smnkl )Tkl or with

Smn = smnkl |E,S Tkl smnkl |E,S = smnkl |E,Θ − (Θ/C)αmn αkl .

Chapter 15 – Crystal thermodynamics. Piezoelectricity

333

Table 15.4: Order of magnitude of the principal and crossed eﬀects deﬁned in this chapter, expressed in International System (SI) units ΔΘ

Ei

Tkl

ΔS

(C/T ) 104

p 10−6

[α] 10−5

Dj

p 10−6

ε0 [ε] 10−10

[d] 10−12

Smn

[α] 10−5

[d] 10−12

[s] 10−11

Table 15.4 allows us to calculate the order of magnitude of the diﬀerence between these isothermal and adiabatic coeﬃcients, viz. 10−4 . 10−5 . 10−5 = 10−14 , while smnkl |E,Θ is on the order of 10−11 , thus larger by three orders of magnitude. The diﬀerence is negligible. This kind of calculation can be performed for all the other tensors, considered under various conditions. For example the diﬀerence between the zero electric ﬁeld and the zero induction elastic constants, with both measurements performed at constant temperature, can be calculated. Generally, the relative diﬀerence between these two coeﬃcients is much smaller than 1. This is not the case for the pyroelectric vector measured at zero stress, denoted by pi |Tkl =0 , and at zero strain, pi |Skl =0 , the electric ﬁeld being zero in either case. At zero stress and electric ﬁeld, Equation (15.17b) can be written as: Pj = pj |Tkl =0 ΔΘ. For a temperature variation ΔΘ at zero strain, Smn = 0, the stress Tkl is no more zero. It is given by Equation (15.17c): 0 = αmn ΔΘ + smnkl Tkl .

(15.29)

To obtain the value of Tkl from this equation, we use the contracted notation for Tkl and αmn in order to use the elastic coeﬃcients under the contracted form sμν , and the matrix c inverse to matrix s. Equation (15.29) can be written, for each value of β, as sβν Tν + αβ ΔΘ = 0.

(15.30)

The matrix of compliance components {sβν } is the inverse of the matrix {cλμ } of stiﬀness components, which translates into relation sβν cνμ = δβμ .

(15.31)

We multiply Equation (15.30) by cμβ , then sum the six equations, with β varying over the range 1 to 6. We obtain: cμβ sβν Tν + cμβ αβ ΔΘ = 0. Using relation (15.31), the ﬁrst term in this equation is equal to δμν Tν = Tμ , and we obtain Tμ = −cμβ αβ ΔΘ

334

Symmetry and Physical Properties of Crystals

so that Tkl = −cklmn αmn ΔΘ equivalent to (15.29). Equation (15.17b) becomes Pj = pj |Tkl =0 ΔΘ − djkl cklmn αmn ΔΘ = pj |Skl =0 ΔΘ. We obtain: pj |Skl =0 = pj |Tkl =0 − djkl cklmn αmn . The diﬀerence between the two pyroelectric eﬀects is, according to Table 15.4, on the order of 10−6 , i.e. on the same order as the pyroelectric eﬀect. This means that the pyroelectric vector at zero strain is diﬃcult to measure, because it is extremely small. It is called primary pyroelectricity, while the term djkl cklmn αmn which is to be added to obtain the pyroelectric vector at constant stress is called secondary pyroelectricity. If the crystal is not submitted to stress during the change in temperature, it is free to deform through thermal expansion. This deformation produces, through piezoelectricity, a polarization which is secondary pyroelectricity.

15.5. Exercises Exercise 15.1 Show that all the components of the piezoelectric tensor for group 432 are zero although this group is not centrosymmetric. Use the tensor form given in Table 15.2 for group 422, a subgroup of 432, and supplement it with the additional symmetry operation that leads to group 432. Exercise 15.2 Consider a crystal with point group ¯42m, assuming the form of the tensor is known for one of its subgroups, 222 or mm2. Choose the axis Ox3 parallel to the ¯4 axis. 1.

Determine the non-zero coeﬃcients of the piezoelectric tensor in the two following cases: (a) Ox1 is chosen parallel to one of the 2-fold axes, (b) Ox1 is chosen perpendicular to one of the mirrors.

2.

The compound (NH4 )H2 PO4 (ammonium dihydrogen phosphate, ADP), with point group ¯42m, has, in the axis system deﬁned in question (1a), the piezoelectric coeﬃcients: d14 = d25 = 0.17 × 10−11 C N−1 and d36 = 5.17 × 10−11 C N−1 . Determine its piezoelectric coeﬃcients in the axis system deﬁned in question (1b).

Chapter 15 – Crystal thermodynamics. Piezoelectricity

335

Exercise 15.3 Show that the longitudinal piezoelectricity surface for a crystal with point group 422 vanishes for all directions. (A similar result would be obtained for group 622). The form of the piezoelectric tensor for group 422 is given in Table 15.2. Exercise 15.4 Quartz SiO2 belong to group 32, for which the form of the piezoelectric tensor is given in Table 15.2 for the axis system where Ox3 is parallel to the 3-fold axis and Ox1 is parallel to a 2-fold axis. 1.

A uniaxial stress T is applied to a quartz crystal along a direction in the plane (Ox1 , Ox2 ). Call θ the angle between the direction of the stress and axis Ox1 . (a) Show that the obtained polarization P has a norm independent of θ. (b) How does the direction of P vary when θ varies? (c) What uniaxial stress should be applied to the crystal in order to obtain a polarization along Ox2 ?

2.

Calculate the longitudinal piezoelectric coeﬃcient for a general direction. Represent the intersection of this surface with the plane (Ox1 ,Ox2 ). Deduce the overall look of the longitudinal piezoelectric surface.

Exercise 15.5 Zinc sulﬁde ZnS is a cubic crystal with point group ¯43m. 1.

A rectangle parallelepiped with sides parallel to the vectors a, b and c of the unit cell is cut out of this crystal. What stress (or stresses) should be applied onto this parallelepiped to determine the value of d14 ?

2.

Calculate the longitudinal piezoelectric coeﬃcient in a general direction deﬁned by its direction cosines s1 , s2 , s3 . Express it as a function of the spherical coordinate angles θ and ϕ.

3.

Calculate the values of ϕ and θ for which the longitudinal piezoelectric coeﬃcient is maximum.

4.

A cube of ZnS with sides parallel to directions [110], [¯110] and [001] is submitted to a uniform electric ﬁeld E, parallel to [001]. The value of this ﬁeld is 5 × 105 V m−1 . (a) Show that the volume variation of the crystal under the eﬀect of the applied electric ﬁeld is zero. (b) Determine the relative variation in the lengths of the sides of the cube. The value of d14 is 2 × 10−11 C N−1 .

336

Symmetry and Physical Properties of Crystals

Exercise 15.6 1.

Quartz, with point group 32, is piezoelectric. We try to predict, using Curie’s principle, whether the application of a uniaxial stress along some simple crystallographic directions can lead to a polarization. Consider in turn the cases where: (a) the uniaxial stress is parallel to the 3-fold axis, (b) the uniaxial stress is parallel to a 2-fold axis, (c) the uniaxial stress is parallel to Ox2 , with Ox1 being parallel to the 2-fold axis of (b), (d) the stress is a shear T12 .

2.

Zinc oxide ZnO, with point group 6mm, is piezoelectric. We discuss the same questions as in (1), viz. whether a polarization can exist under the inﬂuence of a uniaxial stress. We choose an orthonormal axis system where Ox3 is parallel to the 6-fold axis and Ox1 is perpendicular to one of the mirrors. Consider the following cases: (a) the uniaxial stress is parallel to Ox3 , (b) the uniaxial stress is parallel to Ox1 , (c) the uniaxial stress is parallel to Ox2 . For each case, check the results by using the appropriate piezoelectric tensor, as given in Table 15.2.

Exercise 15.7 Consider a crystal with point group ¯42m. Choose an orthonormal axis system (Ox1 x2 x3 ) where Ox1 and Ox2 are parallel to the 2-fold axes. Using Curie’s principle, determine whether a shear stress T12 allows a polarization to exist. Same question if the shear stress rotates by 45◦ around axis Ox3 . Check the obtained results by using the piezoelectric tensor for group ¯42m.

Chapter 15 – Crystal thermodynamics. Piezoelectricity

337

Complement 15C. Electrostriction and magnetostriction Piezoelectricity is discussed in Section 15.3. It relates, through Sij = dijk Ek , an electric ﬁeld with the strain, linear with respect to the ﬁeld, which it produces or, conversely, it relates the stress to the electrical polarization, again with a linear dependence. It is present only in crystals belonging to some point groups, and in particular lacking a center of symmetry. Electrostriction is more general a property. It relates an electric ﬁeld with the strain it produces, but now the strain is proportional to the square of the electric ﬁeld in the case of an isotropic material, or bilinear in the ﬁeld components for an anisotropic material: Sij = Qijkl Ek El . This property, represented by a rank-4 tensor, is featured by all insulating materials (dielectrics), including liquids and crystals of any symmetry, but its intensity varies considerably. Piezomagnetism, the magnetic analogue of piezoelectricity, was long believed to be impossible, until this was shown to be wrong in the late 1950’s. It is however a weak eﬀect, and is restricted to materials with special (magnetic) symmetry, such as the antiferromagnets MnF2 , CoF2 and NiF2 . Magnetostriction is the magnetic eﬀect roughly corresponding to electrostriction. It too varies considerably among materials. Large eﬀects are encountered in ferro- or ferrimagnets, i.e. materials which have, at the microscopic level, an ordered magnetic structure. The main contribution is due to the growth, under an applied magnetic ﬁeld, of the domains7 with magnetization direction near that of the ﬁeld; at saturation, the strain is the spontaneous magnetostrictive strain, whereas the demagnetized state as well as the zero-ﬁeld state involve an average over the domain magnetization directions. The most eﬃcient magnetostrictive material is Terfenol D, a rare-earth–iron compound with formula8 Tbx Dy1−x Fe2 , with x ∼ 0.3, in which strains of the order of 2 × 10−3 are encountered. Both magnetostrictive and electrostrictive materials are important for applications, the more obvious ones being sensors and actuators. One of the advantages of the magnetic version is the fact that a magnetic ﬁeld can be applied through external coils and magnetic circuits, and does not require voltage to be applied on the actuator or sensor itself.

7. See the footnote in Complement 8C. 8. The “nol” at the end of Terfenol has nothing to do with the international organic chemistry nomenclature, which links “ol” to alcohols: it just celebrates the (U.S.) Navy’s Ordnance Laboratory, where research on magnetostrictive materials has long been very active toward the development of sonar for underwater sensing.

338

Symmetry and Physical Properties of Crystals

Further reading E. du Trémolet de Lacheisserie, D. Gignoux and M. Schlenker (ed.), Magnetism, vol. 1: Fundamentals (Springer Verlag, New York and Heidelberg, 2005), chap. 12 E. du Trémolet de Lacheisserie, D. Gignoux and M. Schlenker (ed.), Magnetism, vol. 2: Materials and Applications (Springer Verlag, New York and Heidelberg, 2005), chap. 15

Chapter 15 – Crystal thermodynamics. Piezoelectricity

339

References [1] L.D. Landau, E.M. Lifshitz and L.P. Pitaevskii, Course of Theoretical Physics, vol. 8, Electrodynamics of Continuous Media, 2nd edn. (Elsevier, Oxford, 1984) [2] H.B. Callen, Thermodynamics and an Introduction to Thermostatistics, 2nd edn. (Wiley, New York, 1985) [3] J.F. Nye, Physical Properties of Crystals: Their Representation by Tensors and Matrices (Oxford University Press, Oxford, 1985) [4] Landolt and Börnstein Tables, vol. III.2 (Springer Verlag, Berlin, 1969)

Chapter 16

Light propagation in crystals When an electromagnetic wave propagates in a crystal, the material becomes electrically polarized by the electric ﬁeld of the wave since its electrical permittivity is diﬀerent from that of vacuum. The propagation of electromagnetic waves is governed by Maxwell’s equations. In the case of anisotropic materials, these yield the birefringence of crystals, which is thoroughly discussed.

16.1. Maxwell’s equations Assuming an uncharged, non-conducting material, Maxwell’s equations have the form: div D = 0 curl E = −

E

(16.1a) ∂B ∂t

div B = 0 ∂D curl H = ∂t

(16.1b) (16.1c) (16.1d)

where D is the electrical induction deﬁned in (15.3) and again here in (16.3), the electric ﬁeld, B the magnetic induction, H the magnetic ﬁeld. Since we consider non-magnetic materials: B = μ0 H where μ0 is the magnetic permeability of vacuum (μ0 = 4π × 10−7 in SI units), hence div H = 0

(16.1e)

∂H . (16.1f) ∂t Dielectric materials polarize under the inﬂuence of an oscillating electric ﬁeld E. The polarization P is related to the electric ﬁeld by relation: curl E = −μ0

P = ε0 [χ]E © Springer Science+Business Media Dordrecht 2014 C. Malgrange et al., Symmetry and Physical Properties of Crystals, DOI 10.1007/978-94-017-8993-6_16

(16.2)

341

342

Symmetry and Physical Properties of Crystals

where [χ] is the electrical susceptibility tensor of the material, in the linear approximation which we adopt throughout this chapter. The materials for which this approximation is suﬃcient are linear materials. Induction D is then given by: D = ε0 E + P = ε0 E + ε0 [χ]E = ε0 [ε]E. (16.3) ε0 is the permittivity of vacuum (1/4πε0 = 9×109 in SI units) and [ε] = [E]+[χ] is the tensor of relative permittivity of the material, with [E] the unit tensor. This equation was already given in (15.3), in the discussion of permittivity in a static electric ﬁeld. Here the electric ﬁeld is rapidly variable, and the values of the coeﬃcients of the relative permittivity tensor [ε] can be very diﬀerent from their value for a static ﬁeld. If the material is isotropic, tensor [ε] reduces to a scalar, and the propagation equation for an electromagnetic wave is easily solved since condition (16.1a) then leads to div E = 0. The solution for anisotropic materials is more complicated, and we restrict our search to sinusoidal solutions. Also, we here consider only transparent materials, i.e. non absorbing materials, hence the components of tensor [ε] are assumed to be real.

16.2. Light propagation in an isotropic material We discuss propagation in either vacuum or an isotropic dielectric for which tensor [ε] is a scalar, noted ε. Using Maxwell’s equations, we calculate: curl curl E = −μ0

∂ ∂2D ∂2E (curl H) = −μ0 2 = −μ0 ε0 ε 2 ∂t ∂t ∂t

and we then use the identity: curl curl E = grad div E − ΔE. Since D and E are parallel (this will no more be the case in an anisotropic material), div E = 0 from (16.1a), and we obtain: ΔE − ε0 μ0 ε

∂2E = 0. ∂t2

(16.4)

This equation has solutions of the form: s · r (16.5) E = E0 f t ± v √ with v = 1/ εε0 μ0 , i.e. plane waves propagating in the direction of unit vector s at velocity ± v (see (14.6) and Fig. 14.1). t±

Setting si ∂f ∂E = ±E0 , ∂xi v ∂u

s·r = u, v ∂2E s2 ∂ 2 f = E0 i2 2 , 2 v ∂ u ∂xi

∂2E ∂2f = E0 2 2 ∂t ∂ u

Chapter 16 – Light propagation in crystals

343

and Equation (16.4) is veriﬁed if 1/v 2 = εε0 μ0 . In vacuum, ε = 1 and v = c. We ﬁnd the well-known relation ε0 μ0 c2 = 1. √ We deduce that, in a dielectric material, v = c/ ε. By deﬁnition, the optical index, or refractive index, of a material is n = c/v, and the above relations indicate that n2 = ε. We would of course have obtained the same solution for the magnetic ﬁeld, i.e. √ a plane wave propagating at velocity v = c/ ε.

16.3. Sinusoidal waves that are solutions of Maxwell’s equations Plane sinusoidal waves have the form: E = E0 cos(k · r − ωt)

E = E0 [exp i(k · r − ωt)]

or

(16.6)

where k = ks is the wave vector, ω is the angular frequency of the wave, and means “real part of”. We can write: cos(k · r − ωt) = cos[ω(t − ks · r/ω)]. Comparing with Equation (16.5), we see that the propagation velocity v, or phase velocity, is such that: ω (16.7) v= . k Furthermore, k · r = ks · r = k (Fig. 14.1) if is the distance from origin of a wave plane, counted along an axis parallel to s. The wavelength λ is such that, for a distance equal to λ, the argument of the cosine varies by 2π, hence λ = 2π/k. Note: if we had chosen, as is customary in crystallography and in X-ray diﬀraction, to express waves in the form cos 2π(k · r − νt) (Tab. 3.1), the norm of the wave vector would be equal to 1/λ. The frequency ν is equal to ω/2π. The sinusoidal behavior of vectors E and H makes the diﬀerentiations of vectors E or H with respect to time and to the coordinates very easy: ∂E = −i ω E, ∂t

div E = i k · E

and

curl E = i k × E.

(16.8)

The same relations are valid for vector H. Applying these relations to Equations (16.1a) and (16.1e), we obtain: k·D=0

and

k·H=0

(16.9)

so that vectors D and H are perpendicular to wave vector k. Furthermore, we deduce from Equations (16.1d) and (16.1f): k × H = −ωD,

(16.10a)

k × E = μ0 ωH.

(16.10b)

344

Symmetry and Physical Properties of Crystals

Vector D is perpendicular to H and to k from (16.10a), and H is perpendicular to k after (16.10b). We deduce that vectors k, D and H form a direct trirectangular trihedron, whether the material is isotropic or not (Fig. 16.1a). Furthermore, E is perpendicular to H (16.10b), and therefore lies in the plane deﬁned by D and k. In an isotropic material, the trihedron deﬁned by k, E and H is also a direct trirectangular trihedron (Fig. 16.1b). H

H

E

s k

D

u

k

E D

S

S

(a)

(b)

Figure 16.1: Relative orientations of vectors H, E, D, S and k. Vector H is perpendicular to the four other vectors. (a) Anisotropic material. (b) Isotropic material. The direction of energy propagation, hence of the light rays, is that of Poynting’s vector S, the norm of which represents the energy that propagates across unit area during unit time, i.e. the intensity of the light beam propagating in the direction of S: S=E×H so that S is perpendicular to E and H. In an anisotropic material, the direction of energy propagation is thus usually diﬀerent from that of the wave vector, and thus the propagation velocity of energy is diﬀerent from the propagation velocity of the wave planes, which is the phase velocity deﬁned in (16.7). In an isotropic material, S is parallel to k. It is then easy to calculate the norm of S, because vectors E, H and S form a trirectangular trihedron. Using relation (16.10b), we ﬁnd: S = E H = kE 2 /μ0 ω = E 2 /μ0 v = ε0 εvE 2 . In an isotropic material, and in particular in air, the intensity of an electromagnetic wave is thus proportional to the square of the norm of the electric ﬁeld.

Chapter 16 – Light propagation in crystals

345

16.4. Plane monochromatic wave in an anisotropic material 16.4.1. Basic equation In an anisotropic material, the polarization P induced by an electric ﬁeld E is, in general, no more parallel to E. It is related to E by the electrical susceptibility tensor [χ]: P = ε0 [χ]E and

D = ε0 E + P = ε0 ([E] + [χ])E = ε0 [ε]E.

(16.11)

[ε] is the relative permittivity tensor of the crystal. This tensor is symmetric (Sect. 15.1.3). Condition div D = 0 does not lead to zero divergence for E any more, and the propagation equation obtained in (16.4) is no more valid. To simplify the problem, we seek, for the electromagnetic wave, a sinusoidal solution, so that the results of Section 16.3 can be used. We saw that the trihedron D, H, k is trirectangular. Vectors E and D are no more parallel, but enclose an angle ϕ. Since E is perpendicular to H, it is in the plane deﬁned by D and k (Fig. 16.1a). Poynting’s vector is perpendicular to E and H. It is therefore also in plane (D, k) and encloses with vector k the same angle ϕ. Using Equations (16.1b) and (16.1d), we obtain: curl curl E = −μ0

∂2D . ∂t2

(16.12)

Relations (16.8) make it possible to write Equation (16.12) in the form −k × k × E = ω 2 μ0 D.

(16.13)

Furthermore, we know that any three vectors satisfy relation: A × B × C = (A · C)B − (A · B)C

(16.14)

so that Equation (16.13) becomes: −k(k · E) + k 2 E = ω 2 μ0 D. Since the propagation velocity v of the wave (the phase velocity) is such that v = ω/k (Eq. (16.7)) and since the refractive index is deﬁned by n = c/v, so that n = ck/ω and ε0 μ0 c2 = 1, we deduce that k2 /(ω 2 μ0 ) = ε0 n2 . Setting, as before, k = ks, we obtain: D = ε0 n2 [E − s(s · E)] and

2

[ε]E = n [E − s(s · E)].

(16.15a) (16.15b)

346

Symmetry and Physical Properties of Crystals

Equation (16.15b) is actually a system of three equations: [εij + n2 si sj ]Ej = n2 Ei which are linear and homogeneous equations for E1 , E2 and E3 . For such a system to have solutions, its determinant must be zero. By expressing this condition, we obtain a relation giving the value of index n as a function of the propagation direction s. Because calculating the determinant is tedious, we will use some calculational tricks which lead to the result more easily. We start from Equation (16.15a), and use the fact that D · s = 0.

16.4.2. Birefringence The second-rank, real and symmetric tensor [ε] has three mutually orthogonal principal axes (Sect. 10.2.2). In the coordinate system of these principal axes, the tensor is diagonal: ⎞ ⎛ ε1 ⎠ ⎝ ε2 ε3 and, in the same frame, the components Di and Ei of D and E respectively are related through: D1 = ε0 ε1 E1 ,

D2 = ε0 ε2 E2,

D3 = ε0 ε3 E3 .

(16.16)

Equation (16.15a), when projected onto principal axis Ox1 , yields, using (16.16):

n2 = −s1 (s · E) D1 1 − ε1 ε1 s1 or D1 = − (s · E). (16.17a) ε1 − n2 In the same way, we obtain: ε2 s2 (s · E), ε2 − n2 ε3 s3 D3 = − (s · E). ε3 − n2 D2 = −

(16.17b) (16.17c)

Multiplying (16.17a) by s1 , (16.17b) by s2 and (16.17c) by s3 , and adding them, we obtain for the left-hand side Di si = D · s = 0, hence s2 εi i = 0. εi − n2

(16.18)

i

Expanding (16.18) yields: s21 ε1 (ε2 − n2 )(ε3 − n2 ) + s22 ε2 (ε3 − n2 )(ε1 − n2 ) +s23 ε3 (ε1 − n2 )(ε2 − n2 ) = 0.

(16.19)

Chapter 16 – Light propagation in crystals

347

This equation f (n2 ) = 0 is a second-degree equation for n2 . It is easy to show that it has two solutions. We rank the values of εi in increasing order, for example ε1 < ε2 < ε3 . The value of f (n2 = ε1 ) is positive, that of f (n2 = ε2 ) is negative and that of f (n2 = ε3 ) is positive. The continuous function f (n2 ) therefore goes to zero for two values of n2 , one between ε1 and ε2 , the other between ε2 and ε3 . One value of n2 corresponds to a single value of n, because a negative index would be equivalent to a negative velocity, simply describing a wave propagating the other way. This is why only positive indices are considered. For a given propagation direction, there are thus two values of the refractive index, hence two waves can propagate: they are called the eigenmodes. The material is said to be birefringent, or one says there is birefringence. From now on, we set: n1 =

√

ε1 ,

n2 =

√

ε2 ,

n3 =

√

ε3

(16.20)

and n1 , n2 and n3 are called the principal indices (meaning the indices associated to the principal values of tensor [ε]).

16.4.3. Index surface The index surface is the locus of points M such that OM = n s, where n is the value of the index for a wave with wave-vector parallel to unit vector s.1 Since there are two values of n for one propagation direction s, the index surface intersects any radius vector at two points. Biaxial materials We saw (Sect. 10.5) that symmetric rank-2 tensors, representing physical properties of triclinic, monoclinic or orthorhombic crystals, have three principal values which normally are diﬀerent. Therefore, for such crystals, ε1 = ε2 = ε3 , and we obtain an index surface as shown on Figure 16.2a, where only oneeighth of the surface is represented because this surface is symmetrical with respect to planes s1 = 0, s2 = 0 and s3 = 0. If s1 = s2 = 0, and therefore s3 = 1, Equation (16.19) leads to n2 = ε1 √ and n2 = ε2 . The index surface intersects axis Ox3 at x3 = ε1 = n1 and √ √ x3 = ε2 = n2 . In the same way, it intersects axis Ox1 at x1 = ε2 = n2 and √ √ √ x1 = ε3 = n3 and axis Ox2 at x2 = ε3 = n3 and x2 = ε1 = n1 . It is easy to show that the intersections of the index surface by the planes xi = 0 corresponding to si = 0 consist of a circle and an ellipse. These curves do not intersect in planes x1 = 0 and x3 = 0, but they do intersect in plane x2 = 0. Because of the symmetry of the index surface, there are in this plane four points of intersection, deduced from one another by symmetries with respect 1. The index surface is also called the wave vector surface when the length along s is taken equal to kn instead of n, k being the modulus of the wave vector in vacuum.

348

Symmetry and Physical Properties of Crystals x3

x3

n2 n1

I

I

x1

n3

n3

n1

O

I’’’

x2

n2

x1

O I’

(a)

I’’

(b)

Figure 16.2: Index surface in the general case. (a) Intersection of the surface with the planes of the orthonormal trihedron formed by the principal axes of tensor [ε]. We assume ε1 < ε2 < ε3 so that n1

s21 ε1 (ε3 − n2 ) + s22 ε1 (ε3 − n2 ) + s23 ε3 (ε1 − n2 ) = 0, hence ε1 (ε3 − n2 )(s21 + s22 ) + ε3 (ε1 − n2 )s23 = 0 and ε1 ε3 − n2 ε1 (s21 + s22 ) − n2 ε3 s23 = 0.

The index surface is deﬁned as the locus of the ends of vectors r such that r = ns, hence xi = nsi . Hence the equation of the second surface is given by: ε1 (x21 + x22 ) + ε3 x23 = ε1 ε3 , or or again

x21 + x22 x23 + = 1, ε3 ε1 x21 + x22 x2 + 32 = 1. 2 ne no

Chapter 16 – Light propagation in crystals

349

This is an ellipsoid of revolution around direction Ox3 , and tangent to the ordinary sphere along axis Ox3 (Fig. 16.3). The two optical axes which were deﬁned for biaxial materials now coincide. There is a single optical axis (whence the name uniaxial crystals), parallel to the n-fold rotation axis with order n larger than 2 (which itself is parallel to basis vector c). If ne > no , the crystal is said to be uniaxial positive (Fig. 16.3a), and if ne < no it is uniaxial negative (Fig. 16.3b). x3

x3 no

no ne

ne x2

x2

(b)

(a)

Figure 16.3: Index surface of a uniaxial crystal. Axis Ox 3 is an axis of revolution. (a) Uniaxial positive crystal. (b) Uniaxial negative crystal. Cubic crystals For cubic crystals, the three principal values of tensor [ε] are equal, and these crystals are isotropic for electromagnetic wave propagation.

16.4.4. Index ellipsoid We will see in the next section that determining the induction vectors D associated to a given propagation direction involves the tensor inverse to [ε] and its associated quadric, called the index ellipsoid, which we now introduce. The relative permittivity tensor [ε] relates E to D/ε0 through: D = [ε]E. ε0

(16.21)

The inverse tensor, called the electrical impermeability tensor, relates D/ε0 to E through: D E =[η] . (16.22) ε0 In the coordinate system of the principal axes of tensor [ε], relation (16.21) takes the form: D2 = ε2 E2 , ε0

D1 = ε1 E1 , ε0 whence

D1 E1 = ε0

1 ε1

= η1

D3 = ε3 E3 , ε0

1 D1 if we set η1 = . ε0 ε1

(16.23)

350

Symmetry and Physical Properties of Crystals

In the same way, we obtain: D2 ε0 D3 = η3 ε0

E2 = η2 E3

1 , ε2 1 with η3 = . ε3 with η2 =

Thus tensors [ε] and [η], inverse to each other, have the same principal axes, and their principal values are reciprocal to each other. The equation of the representative quadric of tensor [η], in the coordinate system of its principal axes, is: η1 x21 + η2 x22 + η3 x23 = 1. The values ηi are always positive since, from (16.23) and (16.20) ηi =

1 1 = 2. εi ni

(16.24)

Hence the quadric is, in all cases, an ellipsoid, called the index ellipsoid. It can also be written as: x22 x23 x21 + + = 1. n21 n22 n23 The semi-axes along the principal axis directions of this ellipsoid are n1 , n2 and n3 . For uniaxial crystals (tetragonal, rhombohedral and hexagonal), the index ellipsoid is of revolution around the axis of order larger than 2 which is always chosen as the Ox3 axis. Earlier, we noted n1 = n2 = no and n3 = ne . The index ellipsoid then has for its equation: x2 x21 + x22 + 32 = 1. 2 no ne

(16.25)

16.4.5. Determining the induction vectors We saw that the induction vector D is perpendicular to the wave vector, hence to unit vector s. If we choose an orthonormal coordinate system (Ox1 x2 x3 ) such that Ox3 is parallel to s, vector D has only two non-zero components, D1 and D2 . They can be obtained by projecting Equation (16.15a), reproduced below, onto the plane (Ox1 x2 ) perpendicular to s. D = ε0 n2 [E − s(s · E)].

(16.15a)

The second term in the right-hand side of this equation has zero projection, and we obtain: Di = ε0 n2 Ei . Also, the projection of Equation (16.22) yields: Dj ε0 Ei = ηij

Chapter 16 – Light propagation in crystals

351

are the components of the electrical impermeability tensor in the where the ηij chosen axis system (which need not be that of the principal axes).

We obtain:

1 D, (16.26) n2 i a system of two linear and homogeneous equations with two unknowns (D1 and D2 ), which is none other than the eigenvector equation of matrix }, a second-rank matrix whose eigenvalues are the values of 1/n2 . {ηij Dj = ηij

The representative surface of tensor [η] is the index ellipsoid. In the subspace formed by Ox1 and Ox2 , the representative surface of this same tensor is the intersection of the ellipsoid by the projection plane, hence an ellipse (Fig. 16.4). Therefore the solutions for D are vectors parallel to the axes of this ellipse. The eigenvalues are the reciprocals of the squares of the half-lengths of the axes of the ellipse (Sect. 10.2.3), hence the values of n are equal to the lengths of the semiaxes of the ellipse. x3 x’3

k O D1 D2

Figure 16.4: Determination of the induction vectors D1 and D2 of a wave with wave vector k, propagating in a birefringent crystal. D1 and D2 are parallel to the axes of the ellipse along which the index ellipsoid intersects the plane normal to vector k and going through the center of the ellipsoid. The lengths of the semiaxes of the ellipse are the values of the respective indices. Conclusion: To ﬁnd the induction vectors of a wave propagating in a crystal with its wave vector parallel to unit vector s, we consider the index ellipsoid of the crystal and its intersection by a plane going through the center of the ellipsoid, and perpendicular to vector s. This intersection is an ellipse. The two waves which can propagate (the eigenmodes) have induction vectors parallel to the axes of this ellipse, and the corresponding indices are equal to the lengths of the semiaxes of the ellipse.

352

Symmetry and Physical Properties of Crystals

Using the index ellipsoid, we can retrieve the results obtained earlier about the existence of one or several optical axes. We demonstrate it for biaxial, then for uniaxial crystals. Biaxial crystals The lengths of the three semiaxes of the ellipsoid are diﬀerent. We again rank them in order of increasing value, n1 < n2 < n3 . The intersections of the ellipsoid by a plane going through the origin are ellipses, but it can be shown that two of these intersections are circles. Consider a wave vector k in the plane (Ox1 , Ox3 ), and enclosing angle β with Ox3 . We look for the ellipse along which the ellipsoid is intersected by the plane perpendicular to k going through O (Fig. 16.5). Its semiaxes are the semiaxis of the ellipsoid parallel to Ox2 , with length n2 , and the radius of the ellipse in plane (Ox1 , Ox3 ) perpendicular to k, with length n . This length n has a value between n1 and n3 , and therefore there is an angle β for which this length is equal to n2 . The ellipse is then a circle, and wave propagation is isotropic. Let k1 be the wave vector thus deﬁned. It is clear, from the symmetry with respect to plane (Ox1 , Ox2 ), that the wave vector k2 , with angle β2 = π − β, also corresponds to a circular section of the ellipsoid. We retrieve the existence of two optical axes and their geometry in the plane perpendicular to Ox2 (Fig. 16.2b). x3 n3 k

n1 x1

O n2 x2

n’

Figure 16.5: Intersection of the index ellipsoid by its planes of symmetry. A wave with wave vector k in plane (Ox 1 , Ox 3 ) has as its indices n2 and n such that n1

Chapter 16 – Light propagation in crystals

353

x3 ne

k

x1

Do no

O

De

n no

x2

Figure 16.6: Determination of the induction vectors of a wave with wave vector k in the case of uniaxial crystals. Axis Ox 3 is parallel to the optical axis and Ox 1 perpendicular to the plane (k, Ox 3 ). We conclude: for uniaxial crystals, the ordinary vibration Do is perpendicular to the optic axis. The extraordinary vibration De is in the plane formed by wave vector k and the optic axis.

16.4.6. Direction of energy propagation The aim of this section is to show that Poynting’s vector is normal to the index surface. We write relations (16.10a) and (16.10b) so that they explicitly show only vectors E and H. k × E = ωμ0 H

(16.27)

k × H = −ωε0 [ε]E.

(16.28)

Consider a variation dk in the wave vector. If the variation is general, it entails not only variations dE and dH, but also dω (dω is zero only if dk is tangent to the index surface). Diﬀerentiating (16.27) and (16.28), we obtain: dk × E + k × dE = ωμ0 dH + μo Hdω,

(16.29)

dk × H + k × dH = −ωε0 [ε]dE − ε0 [ε]Edω.

(16.30)

We dot-multiply (16.29) with H and (16.30) with E after replacing E · [ε]dE by [ε]E · dE, since Ei εij dEj = εji Ei dEj because εij = εji . (H, dk, E) + (H, k, dE) = ωμ0 H · dH + μ0 H 2 dω −(H, dk, E) + (E, k, dH) = −ωε0 [ε]E · dE − E · Ddω. Subtracting both sides of these two equations : 2dk · (E × H) + dE · (H × k − ωε0 [ε]E) −dH · (E × k + ωμ0 H) =(μ0 H 2 + E · D)dω.

(16.31)

354

Symmetry and Physical Properties of Crystals

The second and third terms are zero because of (16.28) and (16.27) respectively, and Equation (16.31) becomes: 2dk · (E × H) = (μ0 H 2 + E · D)dω = 2udω if we note u the electromagnetic energy per unit volume (Born and Wolf, 1980) u=

1 1 (E · D) + (H · B). 2 2

Since we assume the material to be non-magnetic, B = μ0 H. Using the relation that deﬁnes Poynting’s vector, given in Section 16.3, S = E × H, we obtain dk · S = udω. Since S = uvS where vS is the energy propagation velocity, we deduce: vS · dk = dω. The index surface is the constant ω surface in wave vector space. Therefore, if dk has any value in the plane tangent to the index surface, we have dω = 0 and vS is perpendicular to dk. Hence the ray direction, which is the direction of energy propagation vS , is perpendicular to the index surface. We note that E, being perpendicular to vS , is tangent to the index surface.2

16.5. Refraction of a plane wave at the boundary between two materials 16.5.1. The wave-vectors follow the Snell-Descartes law Boundary between two isotropic materials When a wave which propagates in an isotropic ﬁrst material (1) reaches the boundary with a second isotropic material (2), it splits into two waves: one, the refracted wave, propagates in material (2), the other one is reﬂected into material (1). Let E1 , k1 be the electric ﬁeld and the wave vector of the incident wave, E2 and k2 those of the refracted wave, E3 and k3 those of the reﬂected wave. We have:

E1 = E01 exp i(k1 · r − ωt), E2 = E02 exp i(k2 · r − ωt), E3 = E03 exp i(k3 · r − ωt).

The boundary condition on the electric ﬁeld must be satisﬁed at all points on the separation surface and at all times, which implies that the space (and time) 2. The energy propagation velocity, i.e. the group velocity, can be written in the form vS = ∂ω/∂k, a condensed notation for vS1 = ∂ω/∂k1 etc. This is the generalization of the familiar expression for the group velocity in an isotropic material, ∂ω/∂k.

Chapter 16 – Light propagation in crystals

355

variations must be the same. We choose an orthonormal axis system Oxyz so that the origin O is on the separation surface and Oz is perpendicular to this surface. At any point on the surface z = 0, we must therefore have: k1x x + k1y y = k2x x + k2y y = k3x x + k3y y. These equalities must hold whatever the values of x and y. This implies that k1x = k2x = k3x

and

k1y = k2y = k3y .

Thus the tangential component of the wave vector is conserved in refraction and reﬂection. Furthermore, in the isotropic materials we are considering in this section, the rays are parallel to the wave-vectors. This property leads to the Snell-Descartes laws, which have the following expression: 1.

The refracted ray and the reﬂected ray are in the plane of incidence, deﬁned as the plane containing the incident wave vector and the normal to the interface.

2.

The reﬂection angle i3 is equal to the incidence angle i1 . The refraction angle i2 and the incidence angle i1 are related by: n1 sin i1 = n2 sin i2 .

(16.32)

The derivation of these results is straightforward if we look at Figure 16.7a. z

z M3

k1

i1 i3

k3 H material 1 material 2

O i2

i1 i2

k2

M1

M1 M2

M2 (a)

n2

k1

k1

k2

n1

H O

(b)

Figure 16.7: A wave with wave-vector k1 in an isotropic medium 1 gives rise to a reﬂected wave and a refracted wave. (a) Showing the continuity of the tangential component of the wave-vectors at the interface. (b) Construction of the refracted wave-vector k2 when medium 2 is isotropic.

356

Symmetry and Physical Properties of Crystals

The tangential component OH of the incident wave-vector k1 = OM1 is equal to the tangential components of the reﬂected wave-vector k3 = OM3 and of the refracted wave-vector k2 = OM2 . Therefore, vectors k3 and k2 are in the plane of incidence. If n1 and n2 are the indices of materials 1 and 2 respectively, k1 = k3 = k0 n1

and

k2 = k0 n2

where k0 = ω/c is the norm of the wave-vector in vacuum. Also OH = k1 sin i1 = k3 sin i3 = k2 sin i2 . Hence

(16.33)

i1 = i3 , n1 sin i1 = n2 sin i2 .

The above properties make it easy to draw the refracted wave-vector k2 associated to a given incident wave-vector k1 . We draw, starting from point O located on the surface, the vector k1 = OM1 , giving it length n1 (which is equivalent to using k0 as the unit). In medium 2, we draw a half-circle with radius n2 , centered at O. The normal to the interface going through M1 intersects the half-circle with radius n2 at M2 , the end of vector k2 = OM2 . In the following, we will focus solely on the refracted waves. Interface between an isotropic material and an anisotropic material The incident wave, with electric ﬁeld E, gives rise to a reﬂected wave which we ignore, and to two refracted waves, with wave-vectors k2 and k2 , with electric ﬁelds E2 and E2 . This is double refraction. E1 = E01 exp i(k1 · r − ωt), E2 = E02 exp i(k2 · r − ωt), E2 = E02 exp i(k2 · r − ωt). The same argument as above shows that the tangential components of the wave-vectors are continuous at the interface between the two materials, and this leads to the Snell-Descartes laws for the wave-vectors. This is valid for the wave-vectors only, as, in a crystal, the rays are not necessarily parallel to the wave-vectors. The refracted wave-vectors are determined using the same construction as above. As in Figure 16.8, we draw from a point O of the interface, chosen as origin, the incident wave-vector k1 = OM1 , giving it length n1 , i.e. taking as the unit the wave-vector in vacuum k0 . We then draw the two sheets S and S of the index surface, centered at O. The normal to the interface drawn from M1 intersects the index surface at two points M2 and M2 , the ends of wave-vectors k2 and k2 . We thus obtain: n1 sin i1 = n2 sin i2 = n2 sin i2

Chapter 16 – Light propagation in crystals

357

z

k1 i1 O i’2

material 1 crystal

H n1 k1 i2 k2 k’2

M1 S M2

S’

M’2

Figure 16.8: Construction of the wave-vectors of waves which can propagate in a birefringent crystal when the incident wave has wave-vector k1 . S and S are the two sheets of the index surface in the crystal. where angles i1 , i2 and i2 are the incidence angle and the refraction angles for the wave-vectors. If material (1) were anisotropic, the same argument would apply to each of the wave-vectors in material (1), and each wave could give rise to two waves.

16.5.2. Application to uniaxial materials The most frequent applications of crystal birefringence involve uniaxial crystals, for which the index surface consists of a sphere and an ellipsoid of revolution around the optic axis (parallel to the 3-, 4- or 6-fold axis of the crystal). The sphere and the ellipsoid are tangent to each other at their intersection with the optical axis (Fig. 16.3). Several examples will be discussed as a function of the relative orientations of the plane of incidence and the optic axis of the crystal. We assume, for simplicity, that material 1 is isotropic, with index n1 , which makes it easy to draw the index surface related to the incident wave-vector, while retaining the full generality of the argument. We take as the unit for the wave-vectors the value k0 of the wave-vector in vacuum. We recall that the plane of incidence is the plane containing the incident wavevector and the normal to the interface. We deﬁne the principal section plane as the plane containing the optic axis and the normal to the entrance face of the crystal, i.e. the interface between the crystal and material 1, through which light enters the crystal. (a) The optic axis is perpendicular to the plane of incidence The index surface then intersects the plane of incidence along two concentric circles, with radii no and ne (Fig. 16.9a). We obtain two diﬀerent wave-vectors in the crystal. Since the rays are parallel to the normal to

358

Symmetry and Physical Properties of Crystals the index surface, the rays are, in this special case, parallel to the wavevectors. The directions of the corresponding induction vectors are obtained by recalling (see Sect. 16.4.5) that, in a uniaxial material, the ordinary vibration is perpendicular to the optic axis.

(b) The optic axis is parallel to the plane of incidence and to the entrance face The plane of incidence intersects the index surface along a circle for the ordinary surface, and an ellipse for the extraordinary surface (Fig. 16.9b). There are two distinct wave-vectors in the crystal: k2 = OM2 = ko for the ordinary ray, and k2 = OM2 = ke for the extraordinary ray. The ordinary ray is parallel to the ordinary wave-vector, while the extraordinary ray is parallel not to the extraordinary wave-vector but to the normal to the index surface at M2 (vector u on Fig. 16.9b). (c) The optic axis is parallel to the plane of incidence and at any angle to the entrance face This case is represented on Figure 16.9c. The ordinary ray is parallel to the ordinary wave-vector. The extraordinary ray is parallel to the normal at M2 to the index surface (vector u on the ﬁgure). In case (a), the principal section plane is perpendicular to the plane of incidence, while it is parallel to it in cases (b) and (c). In the most general case, the plane of incidence and the principal section plane enclose any angle. This situation is more diﬃcult to represent, because the extraordinary ray is no more in the plane of incidence.

16.6. Conclusion We showed, in this chapter, that crystals which are anisotropic with respect to light propagation (i.e. all crystals except for cubic crystals) are birefringent: an incident plane wave, with given wave-vector, gives rise in the crystal to two waves propagating with two diﬀerent indices and diﬀerent wave-vectors. For each wave, the induction vector D is perpendicular to the wave-vector. At the interface between two materials, the tangential component of the wavevector is conserved, hence a simple construction provides, for a given incident wave, the direction of the wave-vectors in the crystal. The corresponding rays are in general not parallel to the wave-vectors, but they are normal to the index surface. Most applications use uniaxial birefringent crystals (tetragonal or rhombohedral or hexagonal). The index surface then consists of a sphere and an ellipsoid of revolution, tangent to each other at their intersection with the optical axis. The induction vector Do of the ordinary wave is perpendicular to the optic axis and the induction vector De of the extraordinary wave is in the plane containing the extraordinary wave-vector and the optical axis.

Chapter 16 – Light propagation in crystals

359

z

z n1 no ne

optic axis

optic axis

n1

O

no

O M1

ne no

M’2

Re

M1 M’2 u M2

De

M2

Ro

Ee De

(a)

Re

Ro

(b) z

n1 O

ne no

opti

c ax

is

M1 M’2 u M2

Ee De Re

Ro

(c)

Figure 16.9: Construction of the refracted rays for a birefringent uniaxial crystal, using the index surface. The incident wave-vector is k1 = OM1 and the refracted wave-vectors are ko = k2 = OM2 for the ordinary wave, and ke = k2 = OM2 for the extraordinary wave. Vectors Do and Eo are always parallel. (a) The plane of incidence is perpendicular to the optic axis. Vectors De and Ee are parallel. (b) The plane of incidence is parallel to the optic axis and the optic axis is in the plane of the surface. (c) The plane of incidence is parallel to the optic axis, which encloses a non-zero angle with the surface of the crystal. In cases (b) and (c), we note that the extraordinary ray Re is parallel to the normal to the index surface at point M2 , and that De is perpendicular to wave-vector ke (while Ee is perpendicular to the ray Re ).

360

Symmetry and Physical Properties of Crystals

In this chapter, we assumed the permittivity of crystals to be real, which means that the crystals are not absorbing. This assumption of perfectly transparent crystals will be retained in all what follows. We make an exception for Figure 16.10, which shows a commonplace evidence of the anisotropic optical properties of zinc crystals, which are often large and conspicuous on zinc-plated metal surfaces, such as lamp poles or sign posts. The very fact that the crystals are visible with the naked eye is due to the dependence of the reﬂectivity on the crystal orientation of the surface.

Figure 16.10: A lamp pole surface, where the crystals comprising the zinc plating are conspicuous because of the anisotropic reﬂectivity of uniaxial zinc. The ribbon in the lower half is a centimeter scale. The contents of this chapter make it possible to solve all problems dealing with light propagation in anisotropic crystals. We therefore thought it unnecessary to make the presentation more cumbersome by adding another approach, which uses the wave surface and the appropriate geometrical construction. This alternative presentation is given in Appendix 16A for the sake of those readers who are used to this approach for isotropic materials and would prefer to use it for anisotropic crystals too.

16.7. Exercises Throughout the exercises for this chapter, the prisms are assumed to be right prisms having a right triangle with apical angle θ for their basis. For simplicity, they are called prisms with angle θ. The ﬁgures show the plane of incidence, which is always perpendicular to the lateral edges of the prism. Exercise 16.1 Calculate the maximum value of the angle δ between the direction of the wave-vector and that of the associated ray in a uniaxial crystal with indices no and ne . Find the numerical value for quartz, with no = 1.544 and ne = 1.553.

Chapter 16 – Light propagation in crystals

361

Exercise 16.2 Consider a parallel-faced slab of calcite (a uniaxial negative crystal, meaning ne < no ), cut so that the optic axis is at 45◦ to the normal to the plate. The ﬁgure below shows the principal section plane of the plate, i.e. the plane containing the normal to the plate and the optic axis. The plate is illuminated by a beam of natural light, monochromatic and perpendicular to the plane of the plate.

45°

1.

Draw the path of the light rays in the plate and after the plate. Indicate their polarization state.

2.

Calculate the deviation Δ between the ordinary and extraordinary rays emerging from the plate, if the thickness e of the plate is 1 cm and the ordinary and extraordinary indices of calcite are respectively 1.6584 and 1.4865.

Exercise 16.3 A transparent uniaxial crystal is cut into a prism with apical angle θ = 30◦ (see ﬁgure below). The optic axis is parallel to the face containing AB and perpendicular to the lateral edge of the prism. A 30°

B

1.

C

This prism is placed on a goniometer so that the entrance face for the beam is the face containing AB, and that this face is perpendicular to the incident beam. Draw the propagation directions of the beams in the prism

362

Symmetry and Physical Properties of Crystals and at the exit of the prism. The deviation δo by the prism for the ordinary beam is 26.02◦ , and the deviation δe of the extraordinary beam is 18.01◦ . Find the values of no and ne .

2.

The prism is rotated around an axis parallel to its lateral side so that the entrance face is the one containing AC, and that it is normal to the incident beam. Draw the ray paths in the prism. Calculate the numerical values of the angular deviations produced by the prism for the ordinary and extraordinary rays.

Exercise 16.4 A Glan-Foucault polarizer consists of two identical prisms with angle θ, with their optic axes parallel to the lateral edges. The prisms are separated by a thin air layer (see the ﬁgure below, where the thickness of this layer is exaggerated). 9

9

The prisms are made of calcite (no = 1.658 and ne = 1.486). The device is illuminated by a monochromatic, unpolarized beam perpendicular to the entrance face. Calculate the range of angles θ such that there is only one beam at the exit of the device. Draw the ray paths in this case, and determine the polarization of the outgoing beam. Exercise 16.5 A calcite prism ABC, with lateral sides parallel to the optic axis, is associated, as shown on the ﬁgure below, with a prism ACD made of glass with index n. The device is illuminated at normal incidence by a monochromatic beam. A

D glass 30°

30° B

9

calcite C

Chapter 16 – Light propagation in crystals

363

1.

Draw the beam paths inside the two-prism system. Indicate the polarization state of each of the two waves at the exit of the two prisms.

2.

Calculate the angle α between the two outgoing beams in the case of calcite, where no = 1.6584 and ne = 1.4865 assuming the glass has index n = 1.55.

Exercise 16.6 A Rochon prism consists of two calcite prisms (ABC and ACD on the ﬁgure below), with angle 30◦ , placed at optical contact so that they form one composite parallel-faced slab. In prism ABC, the optic axis is perpendicular to the entrance face AB. In the second prism, the optic axis is parallel to the lateral edges. The device is illuminated at normal incidence by a monochromatic beam. A

9

D

30°

30° B

C

1.

Draw the ray paths through the two-prism system. Indicate the polarization state for each of the two waves at the exit of the two prisms.

2.

Calculate the angle α between the two outgoing beams in the case of calcite, for which no = 1.6584 and ne = 1.4865.

364

Symmetry and Physical Properties of Crystals

Appendix 16A. Wave surface (or ray surface) and Huygens’ construction 16A.1. Wave surface (or ray surface) It is deﬁned by considering a point source of electromagnetic wave at O. The wave surface is the locus of the points reached by the wave after a given time t, i.e. the equal-phase surface. It is thus the locus of points M such that OM = vS u where vS is the propagation velocity of energy in the direction of unit vector u, parallel to the Poynting vector S. We ﬁrst search for the relation between the phase velocity v of the wave with wave-vector k in the crystal and the energy propagation velocity vS for the same wave. A wave plane P (Fig. 16A.1) moves perpendicular to the wavevector at velocity v, the phase velocity. After a second, it is at P , a distance v from P. During the same time interval, energy propagates from A to B along the direction of the Poynting vector S, with unit vector u. Distance AB is therefore equal to vS . Let ϕ be the angle between vectors k and S. We see that vS =

v . cos ϕ

P

(16A.1)

P’ S u vs

A

s

v k

B H

Figure 16A.1: Propagation of a wave plane from P to P over a time interval of one second. The wave-vector k is normal to P and P . We show that the wave surface can be easily deduced from the index surface because the equation describing the wave surface has a form similar to the equation yielding the index surface. Consider Equation (16.10a) which we reproduce below, and cross-multiply both of its sides with u, using for the left-hand side relation (16.14) for the double cross product: k × H = −ωD u × k × H = k(u · H) − H(u · k) = −H(u · k) because u is perpendicular to H. We deduce that: 1 k 1 1 u × D = − (u × k × H) = (u · k)H = (u · s)H = cos ϕH ω ω ω v

(16.10a)

Chapter 16 – Light propagation in crystals

365

and, using (16A.1), u×D=

1 H vS

and

H = vS (u × D).

(16A.2)

The same process is applied to Equation (16.10b): k × E = μ0 ωH

(16.10b)

u × k × E = k(u · E) − E(u · k) = −kE(u · s) because u is perpendicular to E. u×H = and

k cos ϕ 1 1 E (u × k × E) = − (u · s)E = − E=− μ0 ω μ0 ω μ0 v μ0 vS (16A.3) E = − μ0 vS (u × H).

Using (16A.3), then (16A.2), we obtain: E = −μ0 vS2 (u × u × D) = −μ0 vS2 [u(u · D) − D] so that

E = μ0 vS2 [D − u(u · D)]

(16A.4)

which can be compared to Equation (16.15a), which we repeat: D = ε0 n2 [E − s(s · E)].

(16A.5)

These two equations have the same form. This is even more conspicuous if we rewrite them in order to show E and D/ε0 instead of E and D:

v2 D D (16A.6) E = S2 −u u· c ε0 ε0 and

D = n2 [E − s(s · E)]. ε0

(16A.7)

Equation (16A.7) relates D/ε0 to E by introducing the index n for the wave with wave-vector k parallel to unit vector s and perpendicular to D. The surface n = f (s) is the index surface. On the other hand, D/ε0 and E are related by the permittivity tensor [ε]. Equation (16A.6) relates E to D/ε0 by introducing the propagation velocity of energy vS /c (i.e. this velocity expressed in units of c, the velocity of light in vacuum) in the direction of Poynting’s vector S, parallel to unit vector u and perpendicular to E. The surface v S /c = f (u) is the wave surface. On the other hand E and D/ε0 are related through the impermeability tensor [η]. Thus Equation (16A.6) deduces from (16A.7), which was used throughout this chapter, by replacing D/ε0 by E, E by D/ε0 , s by u and n by vS /c. Although they do not appear directly in the equations, it is clear that tensor [ε] is replaced by [η].

366

Symmetry and Physical Properties of Crystals

This correspondence makes it possible to deduce the equation of the wave surface from that of the index surface, given in (16.18) and expanded in (16.19): i

and

u21 η1

v2 η2 − S2 c

u2i ηi =0 v2 ηi − S2 c

vS2 2 η3 − 2 + u2 η2 η3 − c

vS2 2 + u3 η3 η1 − 2 η2 − c

vS2 vS2 η1 − 2 c2 c 2 vS = 0. c2

Since ηi = 1/εi , the wave surface has the same characteristics as the index surface provided ni is replaced by 1/ni , if the quantity represented is vS /c (or provided ni is replaced by c/ni if the quantity represented is vS ). We thus obtain, for uniaxial crystals, a wave surface consisting of two sheets: a sphere with radius 1/no (the ordinary wave surface), and an ellipsoid (the extraordinary wave surface), with equation: x21 + x22 x23 + =1 η3 η1 or

x2 x21 + x22 + 3 =1 1 1 n2e n2o

if the axis of order larger than 2 (the optic axis) is chosen as Ox3 . This is an ellipsoid of revolution around Ox3 , tangent to the ordinary sphere (Fig. 16A.2). We showed that the normal to the index surface is parallel to Poynting’s vector with unit vector u. In the same way, the normal to the wave surface is parallel to unit vector s, hence to the wave-vector k, and the induction vector D is then tangent to the wave surface. Figure 16A.2 shows the wave surface for a uniaxial material, positive in (a), negative in (b). x3

x3

1/no

1/no 1/ne

1/ne x2

(a)

x2

(b)

Figure 16A.2: Wave surfaces for uniaxial materials when the represented quantity is v S /c: (a) Uniaxial positive; (b) Uniaxial negative

Chapter 16 – Light propagation in crystals

367

16A.2. Huygens’ construction It rests on the Huygens principle, which can be expressed on the basis of envelope waves. Consider a wave surface Σ1 in a given material. One second later, this wave surface has become surface Σ2 , which is the envelope of the wave surfaces emitted by each point of Σ1 . This result applies easily to the transmission of a plane wave from one isotropic material with index n to an anisotropic material. We recall that a wave plane is a wave surface for a point emitter located at inﬁnity. Let AO be the incident ray direction in the isotropic material, and P the wave plane. Let Δ be the line along which the incident wave plane intersects the interface, one second after it went through O. The distance from Δ to plane P is equal to c/n if the isotropic material has index n. The wave plane in the crystal one second after it passed through O goes through line Δ and is tangent to the wave surface emitted at O (Fig. 16A.3). We thus obtain two wave planes, tangent respectively at M and M to the two sheets Σ and Σ of the wave surface. The rays propagate in the crystal along OM and OM . In a completely general case, points M and M are not in the plane of incidence represented on the ﬁgure. A

P c/n

O ’

M’ M

’

R’

R

Figure 16A.3: Use of the wave surface to represent the transmission of a plane wave from an isotropic material into an anisotropic material (Huygens’ construction). We draw the wave planes Π and Π going through line Δ and tangent to the two sheets of the surface. Let M and M be the contact points. The rays are given by directions OM and OM whereas the wave-vectors are perpendicular to the wave planes.

Figure 16A.4 shows the application of this method in two special cases of uniaxial materials. In (a), the optic axis is parallel to the surface and to the plane of incidence. In (b), it has a general direction but the incident ray is perpendicular to the surface.

368

Symmetry and Physical Properties of Crystals P 1/n

optic axis

1/no 1/n O

’

M’ Ee De

op tic

M

’

P

Ro Re

(a)

Ee De

1/no is

ax

Ro Re

(b)

Figure 16A.4: Use of Huygens’ construction to represent the transmission of a plane wave from an isotropic material with index n to an anisotropic uniaxial material (indices no and ne ) in the case when the optic axis is in the plane of incidence. The speed unit is here c as in Figure 16A.2. Ro and Re are the ray directions for ordinary and extraordinary rays, respectively. (a) The optic axis is in the plane of the interface. (b) The optic axis is not in the plane of the interface, and the incident ray is perpendicular to the interface. Line Δ is then at inﬁnity.

Chapter 17

Polarization of light by crystals In this chapter, we show how crystal birefringence can be used to change the polarization of an electromagnetic wave and thus obtain light in a well-deﬁned polarization state. Various devices using this birefringence are described: linear polarizers and phase shifting plates.

17.1. Polarization state of an electromagnetic wave We ﬁrst deﬁne the polarization state for a plane and monochromatic electromagnetic wave propagating in vacuum. We consider the electric ﬁeld vector rather than the magnetic ﬁeld vector because the interaction of this wave with a material, assumed here to be non magnetic (Sect. 16.1), occurs mainly through the electric ﬁeld. The electric ﬁeld of the plane wave in vacuum is perpendicular to the wave-vector. Therefore, if we choose a coordinate system where Oz is parallel to the propagation direction, the electric ﬁeld has only two components, Ex and Ey : Ex = E1 cos(kz − ωt + α)

(17.1)

Ey = E2 cos(kz − ωt + β)

(17.2)

The values of α and β depend on the origins of z and t chosen. Through an appropriate change in either of these origins, we can always obtain: Ex = E1 cos(kz − ωt) Ey = E2 cos(kz − ωt + ϕ)

(17.3) where

ϕ = β − α.

(17.4)

Because the wave is plane, it is suﬃcient to represent the electric ﬁeld E along the propagation direction, Oz. Various cases will be investigated as a function of the value of ϕ.

© Springer Science+Business Media Dordrecht 2014 C. Malgrange et al., Symmetry and Physical Properties of Crystals, DOI 10.1007/978-94-017-8993-6_17

369

370

Symmetry and Physical Properties of Crystals

17.1.1. Linearly polarized wave Assume ϕ = 0 or π. Vector E remains parallel to itself, and encloses with axis Ox an angle θ such that tan θ = E2 /E1 if ϕ = 0, and tan θ = −E2 /E1 if ϕ = π (Fig. 17.1). The polarization is called linear or rectilinear. At a given point on axis Oz, the end of vector E oscillates sinusoidally around O. y E2 =0

O

E1

x

= – E2

Figure 17.1: Linear polarizations obtained when the phase shift ϕ between the two perpendicular components is equal to 0 or to π

17.1.2. Circularly polarized wave Assume ϕ = ±π/2 and E1 = E2 : Ex =

E1 cos(kz − ωt) =

E1 cos ψ

Ey = ∓ E1 sin(kz − ωt) = ∓ E1 sin ψ if we set ψ = kz − ωt. The projection m onto a plane perpendicular to Oz of the end M of the electric ﬁeld vector describes a circle with radius E1 since Ex2 + Ey2 = E12 . At a given time t, ψ varies linearly with z and the end of the electric ﬁeld vector describes a helix with axis Oz. If we consider the upper sign (corresponding to ϕ = π/2), the helix is left-handed and we will say that the polarization is left-circular. If ϕ = −π/2, the helix is right-handed1 and the polarization is right-circular (Fig. 17.2). We note that a right-handed helix is transformed into a left-handed helix by a mirror. At a given point of the propagation axis Oz (z ﬁxed), the end of E describes, in the course of time, a circle. Consider, for simplicity, the situation at z = 0.

1. The screws used in mechanical applications are, except for highly exceptional cases, right-handed helices. The same applies to cork-screws. These right-handed screws and cork-screws penetrate into the material if they are rotated clockwise (“to the right”) as seen by an operator facing the material.

Chapter 17 – Polarization of light by crystals

Right-handed helix

371

Left-handed helix

(a) y M

x

O

z

(b)

Figure 17.2: (a) Representation of a right-handed helix and a left-handed helix for which the envelope is materialized by the generators of a cylinder; (b) representation of the variation, along the propagation direction Oz, of the electric ﬁeld vector of a right-circular wave at a given time. The locus of the ends of these vectors is a right-handed helix. Right-circular polarization (ϕ = −π/2 and the lower sign for Ey ) yields: Ex = E1 cos ωt Ey = −E1 sin ωt. Thus, an observer located at a point with z > 0 (downstream along the propagation direction, hence looking at the source) sees the polarization vector OM rotating clockwise (Fig. 17.3a). Conversely, for left circular polarization, the same observer sees the polarization vector OM rotating counterclockwise (Fig. 17.3b). y

y

M t O

t

x

O

x

M

(a) Right circular

(b) Left circular

Figure 17.3: Representation as a function of time of the end M of the electric ﬁeld vector at a given point for a right (a) and a left (b) circular wave. Axis Oz points in the propagation direction.

372

Symmetry and Physical Properties of Crystals

17.1.3. Elliptically polarized wave Consider the most general case, where E1 , E2 and ϕ have any values. We obtain the curve described by m, the projection of the end M of the electric ﬁeld vector on the plane xOy, if we eliminate (kz − ωt) between Equations (17.3) and (17.4). We obtain: Ex2 Ey2 2Ex Ey cos ϕ + − = sin2 ϕ. E1 E2 E12 E22

(17.5)

This is an ellipse, the axes of which are Ox and Oy if cos ϕ = 0, hence for ϕ = ±π/2. For other values of ϕ, it is easily shown that the axes of the ellipse enclose with axes Ox and Oy respectively the angle θ such that: tan 2θ =

2E1 E2 cos ϕ . E12 − E22

If E1 = E2 , θ equals ±π/4 for all values of ϕ. Figure 17.4 shows the trajectory described by the end of the electric ﬁeld vector at a given point as a function of time, for various values of ϕ.

=0

0 < < /2

= /2

/2 < <

=

=

< < 3/2

= 3/2

3/2 < <

= 2

Figure 17.4: Curves described by the end of the electric ﬁeld vector of a plane wave, at a given point, as a function of time, for various values of the phase shift ϕ between the two orthogonal components. The propagation direction points toward the observer. Note: if we consider an electromagnetic wave in a birefringent crystal, the vector perpendicular to the wave-vector which characterizes the polarization state is the induction vector, and all the above results apply to the components Dx and Dy of induction.

17.1.4. Natural light Classical light sources are made up of atoms oriented in all directions, with each of them emitting polarized light. The waves emitted by the various atoms are mutually incoherent. This is called “natural light” or “unpolarized light”. This light is represented as the sum of two incoherent waves, each of them linearly polarized, with their polarizations in any two perpendicular directions. Usually, light is not completely unpolarized: it is partly polarized.

Chapter 17 – Polarization of light by crystals

373

The polarization state is then conveniently described by the Stokes parameters which are deﬁned in Section 17.5. Here we consider totally polarized light, deﬁned by its two orthogonal components, and sometimes totally unpolarized natural light.

17.2. Jones notation Equations (17.3) and (17.4) can also be written as: Ex = E1 [exp i(kz − ωt)] = [E1 exp i(kz − ωt)] Ey = E2 [exp i(kz − ωt + ϕ)] = [E2 exp iϕ exp i(kz − ωt)] where means “real part of”. The type of polarization depends on the values of E1 , E2 and ϕ. The polarization of the wave is thus perfectly determined by the complex components: Ex = E1 Ey = E2 exp iϕ where ϕ is the phase shift between Ex and Ey . In what follows, we will use this complex notation, called the Jones notation, invented by R. Clark Jones in 1941. The Jones vector of the previous ﬁeld is then:

E1 . E2 exp iϕ The amplitude of the electric ﬁeld is equal to the modulus of this complex vector. If needed, the exact form of the wave is obtained by multiplying these complex components by exp i(kz − ωt) and by taking their real parts. A few examples of Jones vectors are given below, with a and b real numbers:

a . Linear polarization: b The angle θ between the electric ﬁeld and axis Ox is such that tan θ = b/a.

a Right circular polarization: . −ia

a Left circular polarization: . ia These Jones vectors for right circular and left circular polarization would have to be interchanged if the waves were described in the form exp i(ωt − kz). In contrast, the rule given by Figure 17.3 to determine whether the polarization is right-handed or left-handed remains valid whatever the choice made for describing the wave.

374

Symmetry and Physical Properties of Crystals

General polarization:

a b exp iϕ

.

17.3. Linear polarizers A linear polarizer changes any incident light into a linearly polarized light, by acting diﬀerently upon the two orthogonal directions of linear polarization. One category of linear polarizers consists of materials which absorb much more eﬃciently one polarization direction than the perpendicular direction. This is, for example, the case of Polaroid® sheets, consisting of long polymer molecules, oriented by the application of a uniaxial stress and maintained in this orientation by enclosing the polymer in a more rigid plastic foil coating. These special molecules absorb the polarization which is parallel to their long side, and transmit the polarization which is perpendicular. The other category splits the incident light into two beams with mutually orthogonal linear polarizations, retaining only one of the beams. One method is based on reﬂection at Brewster’s angle. If light with any polarization state falls under this incidence angle iB on a material with index n, glass for example, the component polarized parallel to the plane of incidence is not reﬂected. The other component, polarized perpendicular to the plane of incidence, is reﬂected, but only partly because part of the incident intensity is transmitted. This Brewster angle is such that tan iB = n. The other, more eﬃcient method, uses the birefringence properties of crystals. There are two types of such birefringent devices. The ﬁrst type uses total reﬂection of one of the two beams (ordinary (o) or extraordinary (e)) on the exit face of a prism, and thus allows only one of the two linearly polarized beams to go through. In order for the outgoing beam not to be deviated, two prisms are mounted next to each other, separated by a thin air layer as in the Glan-Foucault prism (Fig. 17.5a and Exercise 16.4) or by an appropriate cement as in the Nicol prism, the oldest device, invented by William Nicol in 1828 (Fig. 17.5b), and described below. The other type of polarizing prism allows both beams to go through, but they diverge at the exit, thus yielding two distinct, linearly polarized beams (Fig. 17.5c and 17.5d, and Exercise 16.6). The Nicol prism (sometimes called nicol) is an assembly of two calcite prisms (calcite is one of the crystal forms of calcium carbonate CaCO3 , also called Iceland spar because the ﬁrst crystals were found in Iceland), cut in a special way. Calcite has point group ¯3m. It is therefore uniaxial, and the optic axis is the 3-fold axis. Calcite crystals feature cleavage planes deduced from one another by the 3-fold symmetry around the optic axis. An Iceland spar crystal is cleaved along these three planes, forming a parallelepiped in which two sides (AB and AD) are equal and the third (AA ) is approximately three times longer than the two ﬁrst sides (Fig. 17.6a). These relationships were calculated so

Chapter 17 – Polarization of light by crystals

375

9 e

9

e

9

o

o

9 (a)

Canada balsam air

(b)

9

9 o

e

9

o 9

9

o

e

e

(c)

(d)

Figure 17.5: Schematic drawing of polarizing devices: (a) Glan-Foucault prism; (b) Nicol prism; (c) Wollaston prism; (d) Rochon prism. These prisms are made of calcite, a uniaxial negative crystal. A

A’

D’ F’

B C

A

A’ F

D

C’

A1

(a)

O9 Ro

B’ C

E

Re

O’ C’

A1

(b)

Figure 17.6: Nicol prism: (a) overall view; (b) principal section plane AA C C (perpendicular to the entrance face ABCD and containing the optical axis AA1 ). Only the extraordinary ray emerges from the exit surface. It is slightly shifted with respect to the incident beam, the direction of which is shown by a dotted line. that the diagonal plane AA C C be perpendicular to face ABCD used as the entrance face, and that it contain the optic axis AA1 . Plane AA C C is thus the principal section plane. The crystal is sawed along plane AFC F , perpendicular to the principal section plane. The two halves are then cemented together using a thin layer of Canada balsam, for which the index N is 1.55, a value between the ordinary index of calcite no = 1.6584 and its extraordinary index ne = 1.4864 (Fig. 17.6b). The incident beam is directed parallel to the large side AA of the prism, so that the incidence plane coincides with the principal section plane. The rays are drawn as in Figure 16.9c. The ordinary ray can be shown by calculation

376

Symmetry and Physical Properties of Crystals

to reach AC with incidence angle 75.7◦ , a value larger than the limiting angle,2 69.2◦ , corresponding to transition from the ordinary index of calcite to that of Canada balsam. It therefore undergoes total reﬂection. The index n for the extraordinary wave is equal to 1.53 (Exercise 16.5) for this orientation of the wave-vector. The extraordinary ray goes through the Canada balsam, then through the second prism, and emerges parallel to the incident beam and slightly shifted. The extraordinary ray is polarized parallel to the principal section plane. It is easy to rotate this polarization, just by rotating the prism around the incident beam.

17.4. Phase-shifting plates Birefringent plates are used to introduce a phase shift between two perpendicular components of an electromagnetic wave. Consider a uniaxial crystal plate, with parallel faces, cut so that the optic axis is in the plane of the plate (Fig. 17.7).

optic axis

no

O 9Eo

air crystal

x

ko ke

ne

Ee

9Eo

z

crystal air

Ee

Figure 17.7: Propagation of the ordinary and extraordinary rays through a phase-shifting plate, a uniaxial plate with the optic axis parallel to its faces Consider an incident beam perpendicular to the plate. The propagation geometry is then very simple. The ordinary and extraordinary wave-vectors are normal to the plate surface. The same applies for the directions of the ordinary and extraordinary rays in the crystal, and also in air at the exit of the plate. The index for the extraordinary ray is equal to ne . For this simple geometry where the ordinary and extraordinary rays are parallel to the corresponding wave-vectors, the electric ﬁeld vector E and induction vector D are parallel, and the polarization vector can be deﬁned by either of these vectors: we choose E. The polarization of the ordinary ray is perpendicular to the optic axis and that of the extraordinary ray is parallel to it. These two orthogonal 2. We recall that the limiting angle il for incidence of a wave on the surface separating a ﬁrst material, with index n1 , from a second material, with index n2 < n1 , corresponds to refraction angle 90◦ (sin il = n2 /n1 ). If the incidence angle is ≥ il , there is no refracted beam: the wave is totally reﬂected.

Chapter 17 – Polarization of light by crystals

377

directions are called the neutral lines of the plate. If we choose Oz parallel to the propagation direction and Ox parallel to the optic axis, the neutral lines of the plate are axes Ox and Oy. Consider an incident plane wave, the electric ﬁeld of which on the entrance face of the crystal (z = 0) has complex components (Sect. 17.2):

E1 exp −iωt . E2 exp iϕ exp −iωt In the plate, this wave gives rise to the ordinary wave, with polarization parallel to Oy, with index no , with the norm of its wave-vector k no , and to the extraordinary wave, with polarization parallel to Ox, with index ne , and with the norm of its wave-vector k ne . We recall that k = ω/c is the modulus of the wave-vector in vacuum. At a distance z from the entrance face, the wave has changed into: Ex = E1 exp i(k ne z − ωt) Ey = E2 exp iϕ exp i(k no z − ωt). At the exit of the plate with thickness e, the components Ey and Ex have an additional phase shift ψ such that ψ = k(no − ne )e, which can also be written: ψ=

2π (no − ne )e. λ

At the exit, the wave is given in Jones notation by:

E1 . E2 exp iϕ exp iψ The sign of ψ depends on the relative values of no and ne , or more precisely on the indices for each of the neutral lines. We thus distinguish the fast neutral line, parallel to the electric ﬁeld which propagates with the larger velocity and therefore the smaller index, and conversely the slow neutral line (smaller velocity and larger index). If Oy is the fast line, then the phase shift ψ is negative.

17.4.1. Half-wave plates These are plates where the thickness is such that the phase shift ψ is equal to (2p + 1)π, with p an integer. Assume the wave incident on the plate is linearly polarized, with components a and b along two orthogonal axes Ox and Oy, respectively parallel to the neutral lines of the plate.

a State before the plate: . b

a a State after the plate: = . b exp iπ −b

378

Symmetry and Physical Properties of Crystals

The vibration which, at the entrance to the plate, enclosed an angle θ with axis Ox such that tan θ = b/a now encloses an angle −θ (Fig. 17.1). A half-wave plate transforms a rectilinear vibration into another rectilinear vibration, symmetric of the ﬁrst one with respect to its neutral lines.

17.4.2. Quarter-wave plates These are plates whose thickness is such that the phase shift is equal to (p + 1/2)π with p an integer, i.e. ± π/2 modulo 2π. These plates make it possible to change linear polarization into circular polarization. Consider linearly polarized light (natural light after passage through a linear polarizer) such that its polarization direction is at 45◦ to the neutral lines of the plates, chosen as the Ox and Oy axes.

a The state before the plate is: a

a a and after the plate: = , a exp −iπ/2 −ia if the neutral line parallel to Oy is the fast line. After the plate, the polarization is right circular (Fig. 17.8). P

Plate

y

y

y F x

S x

x z

Figure 17.8: Schematic representation of a device providing right circular light starting from any incident polarization (generally an unpolarized beam). P is a linear polarizer. The plate is a quarter-wave plate. The fast F and slow S neutral lines are at an angle of 45◦ to the linear polarization transmitted by P. A left circular polarization would be obtained: either by rotating the polarizer by 90◦ or by leaving the polarizer in the same orientation and by rotating the plate by 90◦ , which exchanges the slow and fast axes of the plate and now introduces a phase shift of π/2. Quarter-wave plates are also used to analyse circular polarization. Consider a right-handed circularly polarized wave and let it go through a quarter-wave plate and then through a linear polarizer (called here analyzer) with a polarization direction at 45◦ to its neutral lines (Fig. 17.9). We choose axes Ox and Oy respectively parallel to the fast and slow neutral lines of the quarter-wave plate.

Chapter 17 – Polarization of light by crystals

379

The polarization direction of the linear analyzer makes an angle of 45◦ with the Ox axis. The Jones vector for the right-circularly polarized wave is:

a −ia

and the intensity of the wave is 2a2 . After the quarter wave plate which induces a phase-shift of π/2 between Oy and Ox components, the wave becomes

a a

.

It is linearly polarized with the polarization parallel to the polarization direction of the linear analyzer. The wave is completely transmitted by the polarizer and its intensity is 2a2 . If the incident wave had been a left-handed circularly polarized wave and if it was passed through the same device (quarter-wave plate and linear polarizer at 45◦ to the neutral lines), the transmitted intensity would have been zero. Such a device analyzes the intensity of the right-handed circular polarization. In contrast, the whole left-handed circularly polarized wave would have been transmitted through the same kind of device but with the direction of polarization of the linear polarizer at an angle of 135◦ with the Ox axis. A

Plate y

y S x

y F x

x z

Figure 17.9: Schematic representation of a device which totally transmits right-handed circular polarized radiation and stops left-handed circular polarization

17.5. Partially polarized waves and Stokes parameters The above sections dealt with perfectly monochromatic waves with perfectly deﬁned polarization state, i.e. totally polarized waves. For these waves, the end of the electric ﬁeld vector, at a given point, describes a perfectly deﬁned curve, an ellipse in the general case. This ellipse reduces to a circle for circularly polarized waves, and to a straight line segment for linearly polarized waves. We mentioned that, in contrast, classical light sources emit totally unpolarized waves (Sect. 17.1.4). The end of the electric ﬁeld vector moves randomly in the plane perpendicular to the propagation direction, and has no preferred orientation in this plane.

380

Symmetry and Physical Properties of Crystals

These two cases are the extreme situations of a totally polarized wave and a totally unpolarized wave. In many cases, we deal with a partially polarized wave, consisting of the superposition of monochromatic waves with various polarization states, obtained for instance through reﬂection or scattering, because these mechanisms aﬀect polarization in a way which depends on the incidence and scattering angles. We then deﬁne the polarization state of a wave propagating along direction Oz using the elements of the coherence matrix J:

< Ex Ex∗ > < Ex Ey∗ > Jxx Jxy = J= Jyx Jyy < E y Ex∗ > < Ey Ey∗ > where the angle brackets indicate that we are dealing with the average value of the quantity over all the waves in the beam. The polarization state of the wave is now deﬁned, using these matrix elements, through the Stokes parameters s0 , s1 , s2 and s3 [1] such that: s0 = Jxx + Jyy = < Ex Ex∗ > + < Ey Ey∗ > s1 = Jxx − Jyy = < Ex Ex∗ > − < Ey Ey∗ > s2 = Jxy + Jyx = 2 < Ex Ey∗ > s3 = − i(Jxy − Jyx ) = 2 < Ex Ey∗ > where stands for “real part of” and for “imaginary part of”. It is clear that s0 represents the intensity of the wave, and that s1 represents the diﬀerence between the intensies transmitted by polarizers with polarization directions respectively parallel to Ox and Oy. We now show that s2 represents the diﬀerence between the intensities transmitted by linear polarizers with polarization directions at 45◦ and 135◦ to Ox respectively. For a wave with Jones vector

Ex , Ey the amplitudes transmitted by these polarizers are respectively: √ E(45◦ ) = ( 2/2) (Ex + Ey ) for the polarizer at 45◦ and √ E(135◦ ) = ( 2/2) (Ex − Ey ) for the polarizer at 135◦ . The intensities are respectively: I(45◦ ) = 1/2 (Ex + Ey )(Ex∗ + Ey∗ ) = 1/2 (Ex Ex∗ + Ey Ey∗ + Ex Ey∗ + Ex∗ Ey ) I(135◦ ) = 1/2 (Ex − Ey )(Ex∗ − Ey∗ ) = 1/2 (Ex Ex∗ + Ey Ey∗ − Ex Ey∗ − Ex∗ Ey ) I(45◦ ) – I(135◦ ) = Ex Ey∗ + Ex∗ Ey = 2 (Ex Ey∗ ) and for a partially polarized wave: I(45◦ ) – I(135◦ ) = 2 < Ex Ey∗ > = s2 .

Chapter 17 – Polarization of light by crystals

381

Let us now show that s3 represents the diﬀerence between the intensities of the waves with right-circular and with left-circular polarization. We saw (Sect. 17.4.2) that the intensity of waves with right (respectively left) circular polarization can be measured using a device consisting of a quarter-wave plate and a linear polarizer with polarization direction at an angle of 45◦ (respectively 135◦ ) to the fast neutral line of the quarter-wave plate chosen as Ox axis. The amplitudes of the electric ﬁelds transmitted by these devices are noted E(π/2, 45◦ ) and E(π/2, 135◦ ) respectively. Similarly the transmitted intensities are noted I(π/2, 45◦ ) and I(π/2, 135◦ ) respectively. One gets: √ E(π/2, 45◦ ) = ( 2/2) (Ex + iEy ) and √ E(π/2, 135◦ ) = ( 2/2) (Ex − iEy ) where Ex and Ey are the components of the wave parallel to the directions of the neutral lines of the quarter-wave plate. Hence the transmitted intensities are: I(π/2, 45◦ ) = 1/2 (Ex + iEy )(Ex∗ − iEy∗ ), I(π/2, 135◦ ) = 1/2 (Ex − iEy )(Ex∗ + iEy∗ ). I(π/2, 45◦ ) − I(π/2, 135◦ ) = i (Ey Ex∗ − Ey∗ Ex ) = 2 (Ex Ey∗ ) and for a partially polarized wave: I(π/2, 45◦ ) − I(π/2, 135◦ ) = 2 < Ex Ey∗ > = s3 . The Poincaré coeﬃcients P1 , P2 and P3 are deﬁned as the Stokes parameters normalized by the intensity of the beam, so that: P1 =

s1 , s0

P2 =

s2 s0

and P3 =

s3 . s0

Thus P1 is the linear polarization rate for axis directions Ox and Oy, P2 that for directions at 45◦ and at 135◦ to axis Ox, and P3 the circular polarization rate (the relative diﬀerence between the intensities of right- and left-circularly polarized waves). A completely polarized wave is described by its Jones vector

a b exp iϕ where a and b are real numbers. Then its Stokes parameters are: s0 = a2 + b2 ,

s1 = a2 − b2 ,

s2 = 2 ab cos ϕ and s3 = 2 ab sin ϕ.

Thus, in this case, the four Stokes parameters are not independent, since s20 = s21 + s22 + s23 . For a partially polarized wave, this relation has no reason to be valid. It can be shown that in all cases s20 ≥ s21 + s22 + s23 , the equal sign applying to a totally polarized wave [1]. It can be shown also that the Stokes parameters of

382

Symmetry and Physical Properties of Crystals

a mixture of independent waves are sums of the respective Stokes parameters of the separate waves. The Stokes parameters of a totally unpolarized wave are such that s1 = s2 = s3 = 0. Considering a wave with given Stokes parameters and denoting by a single symbol s the four Stokes parameters s0 , s1 , s2 and s3 , one can write: s = s(1) + s(2) with and

s(1) = s0 − s21 + s22 + s23 , 0, 0, 0 s(2) = s21 + s22 + s23 , s1 , s2 , s3

s(1) represents the unpolarized part of the wave and s(2) the polarized part. Hence, the degree of polarization τ of the original wave, which is equal to the ratio of the intensity of the polarized part to the total intensity, is given by: Ipol s21 + s22 + s23 τ= = . Itot s0 Exercice 17.7 deals with an illuminating, albeit theoretical, partially polarized wave situation.

17.6. Exercises Exercise 17.1 Consider a plate of quartz (a uniaxial positive crystal, ne > no ), with parallel faces, cut so that the optic axis is parallel to the plate. A monochromatic parallel beam, with wavelength λ = 590 nm in vacuum, is incident on the plate, perpendicular to the plate. 1.

Determine the neutral lines of the plate. Choose an orthonormal axis system with Oz parallel to the incident beam and Ox and Oy parallel to the neutral lines of the plate.

2.

What phase shift does the plate introduce between the components parallel to Ox and Oy of an initially linear polarization? Determine the thickness e of the plate required to obtain a quarter-wave plate, then a half-wave plate. We have no = 1.544 and ne = 1.553.

3.

The incident beam is linearly polarized and its polarization is at 45◦ to the neutral lines of the plate. Show that, if the plate is a quarter-wave plate, the beam after the plate is circularly polarized. Is this a right- or a left-circular polarization? If it is right-circular (or left-circular), how should the device be changed to make it left-circular (or right-circular)?

4.

What do we obtain if we place across the path of this circularly polarized beam another quarter-wave plate, identical to the ﬁrst one, with its neutral lines parallel to those of the ﬁrst one?

Chapter 17 – Polarization of light by crystals 5.

383

What is the eﬀect of a quarter-wave plate on natural light?

Exercise 17.2 Consider a quartz plate (quartz is a uniaxial positive crystal, ne > no ), cut parallel to the optic axis, and set between two crossed polarizers, i.e. polarizers with perpendicular polarization directions. A monochromatic parallel beam (with wavelength λ in vacuum) is incident perpendicular to the plate. 1.

The polarization direction of the beam incident on the plate is at angle α to the fast neutral line of the quartz plate. Calculate, as a function of the phase shift ϕ introduced by the plate, the intensity I of the beam after the analyzer.

2.

Choose α = 45◦ . Determine the smallest thickness of the plate that makes it possible to obtain: i)

zero intensity,

ii) maximal intensity. 3.

α is still equal to 45◦ . The initial beam is now white (i.e. polychromatic), and we are interested in wavelengths in the visible range, 0.4 μm < λ < 0.8 μm. What wavelengths are extinguished after the analyzer if e = 0.2 mm? Assume that ne − no varies little with wavelength and is equal to 0.01.

Exercise 17.3 A parallel, monochromatic, linearly polarized beam is normally incident on a birefringent plate, the neutral lines of which are oriented at 45◦ to the rectilinear vibration. The phase shift introduced by the plate between the extraordinary vibration (// Oy) and the ordinary vibration (// Ox) is ϕ. 1.

Show that, after the plate, the vibration is elliptic, the axes of the ellipse being respectively parallel and perpendicular to the direction of the rectilinear vibration.

2.

Calculate the axis ratio of the ellipse.

Exercise 17.4 Using two linear polarizers with known polarization directions, how can the neutral line directions of a birefringent plate be determined? Exercise 17.5 Consider the Nicol prism described in Section 17.3. Figure 17.6b shows its principal section plane, coinciding with the plane of incidence. The angle (AC, AA1 ) between the optic axis and the entrance face is equal to 45◦ , angle (CA, CC ) is 71◦ and angle (C A, C C) is 22◦ . The ordinary and extraordinary indices of calcite are no = 1.6584, ne = 1.4864, and the index of Canada balsam is N = 1.55.

384

Symmetry and Physical Properties of Crystals

1.

Calculate the angle of incidence of the ordinary ray on AC . Show that this ray is totally reﬂected on the Canada balsam.

2.

Determine the direction of the wave-vector, the index and the polarization of the extraordinary ray. Show that it goes through the Canada balsam.

3.

What is the direction of the extraordinary ray in the prism? Show that the outgoing ray is very slightly shifted with respect to the incident beam.

Exercise 17.6 In view of a special optical application (generation of a wave with angular frequency 2ω starting from a wave with angular frequency ω, a process known as Second Harmonic Generation, SHG, see Complement 19C), we need to ﬁnd a direction of the wave-vector k in a birefringent crystal such that n(2ω) = n(ω). Because the index of a material varies with frequency, the solution can be found, in a uniaxial material, by associating the ordinary wave to one frequency and the extraordinary wave to the other one. For a crystal of KH2 PO4 (Potassium dihydrogen phosphate, KDP), which is uniaxial, ﬁnd the angle θ the wave-vector k must enclose with the optic axis so that ne (2ω) = no (ω), taking into account that n(2ω) > n(ω) and ne < no . Useful values are: for λ1 = 694.3 nm (corresponding to ω): no = 1.506 and ne = 1.466, for λ2 = λ1 /2: no = 1.534 and ne = 1.487. Exercise 17.7 1.

We consider a monochromatic wave with Jones vector

a ib in an axis system Oxy, where a and b are positive real numbers. What is, at a given point, the trajectory of the end of the electric ﬁeld vector of this wave? What is its circular polarization rate ?

2.

Same questions for a wave with Jones vector

b ia

3.

We consider the wave formed by the superposition of the two above waves. Determine the Stokes parameters for this wave and its degree of polarization.

References [1] M. Born and E. Wolf, Principles of Optics, 7th edn. (Cambridge University Press, Cambridge, 1999)

Chapter 18

Rotatory power and optical activity Going through some crystals rotates the linear polarization of incident radiation. This phenomenon, known as rotatory power or circular birefringence, is described by a diﬀerence in refractive index for right- and left-hand circular polarization. It is interpreted through the gyrotropy tensor, related to the space dependence of the permittivity tensor. The investigation of this tensor makes it possible to determine what point groups a crystal must belong to in order to feature this property.

18.1. Deﬁnition of the rotatory power of a material Rotatory power was discovered by François Arago in 1811 and Jean-Baptiste Biot in 1812. The ﬁrst theoretical interpretation was given by Augustin Fresnel in 1824. A material features rotatory power if it causes the plane of polarization of linearly polarized light1 to rotate. This property is distinctly diﬀerent from the previously discussed case of linear, or rectilinear, birefringence. It can exist in optically isotropic crystals (cubic crystals) and also in liquids or solutions. We will not deal with the rotatory power of liquids and solutions because they are outside the scope of this book, which focuses on crystalline solids. Also, the diﬀerences in refractive index involved in this phenomenon are much smaller than those corresponding to birefringence. Therefore, clearly evidencing rotatory power in anisotropic materials requires sending the beam parallel to the optic axis in uniaxial crystals (or to one of the two optic axes in biaxial crystals) in order to eliminate the eﬀect of birefringence.

1. The plane of polarization is the plane containing the wave-vector and the polarization vector, which is perpendicular to it. In a birefringent crystal, the polarization vector is the induction vector D, while in air, where the electric ﬁeld and induction are parallel, the description is based on the electric ﬁeld.

© Springer Science+Business Media Dordrecht 2014 C. Malgrange et al., Symmetry and Physical Properties of Crystals, DOI 10.1007/978-94-017-8993-6_18

385

386

Symmetry and Physical Properties of Crystals

Consider a material featuring rotatory power, for example a quartz plate in which the faces are perpendicular to the 3-fold axis. We illuminate this plate with a linearly polarized beam perpendicular to the plate. After going through the plate, the polarization has rotated by an angle α. This angle turns out experimentally to be proportional to the thickness e of the crystal. The rotatory power ρ is deﬁned by: α ρ= . (18.1) e If we exchange the entrance and exit faces of the plate, the polarization rotation angle α does not change sign. The sign of the rotation angle depends on the crystal, which may be either dextrogyre (rotation to the right) or levogyre (rotation to the left). This requires deﬁning what is meant by rotation to the right or to the left. A crystal is said to be dextrogyre if, for an observer looking at the source through the crystal, the plane of polarization of the light rotates to the right, i.e. clockwise (Fig. 18.1). crystal source

observer

Figure 18.1: Rotation of the induction vector to the right for an observer looking at the source The end of the polarization vector then describes, during propagation in the dextrogyre crystal, a left-handed helix (see Fig. 17.2). It was agreed to give positive values to α for dextrogyre materials. To indicate the order of magnitude of the rotatory polarization phenomenon, Figure 18.2 shows the value of the rotatory power ρ for quartz as a function of the wavelength of light in the visible range. We see that ρ is of the order of a few tens of degrees per millimeter of thickness traversed.

18.2. Fresnel’s interpretation Fresnel interpreted this phenomenon by showing that, if a material has diﬀerent refractive indices for right- and left-hand circular polarizations, then this material shows rotatory power. A linearly polarized electromagnetic wave can be split into two waves with equal amplitudes, one right-circular, the other left-circular. A wave propagating along Oz and polarized along Ox can be split, using the Jones notation (Sect. 17.2), in the following way:

1 1 1 1 1 + . = i 0 2 2 −i

Chapter 18 – Rotatory power and optical activity

387

60

[degree mm–1]

50 40 30 20 10 0 350

400

450

500

550

[nm]

600

650

700

Figure 18.2: Rotatory power of quartz as a function of wavelength The ﬁrst term represents a left-circular vibration, and the second term a right-circular vibration (Sect. 17.2), when using waves with the form [exp i(kz − ωt)]. If the index of the material for the right-circular vibration, nr , is diﬀerent from the index, nl , for the left-circular polarization, the initial wave, with wave-vector in air k0 = 2π/λ, becomes after propagating over a distance z in the crystal:

1 1 1 1 exp(ik0 nl z) + exp(ik0 nr z) i 2 2 −i

1 k0 (nl + nr )z = exp i 2 2

k0 (nr − nl )z k0 (nl − nr )z 1 1 + exp i . × exp i −i i 2 2 We set:

k0 (nl + nr )z k0 (nr − nl )z =ψ and = α . 2 2 We obtain a vibration:

1 cos α exp −iα + exp iα = exp iψ exp iψ i exp −iα − i exp iα sin α 2 i.e. a linearly polarized vibration, with polarization at an angle α with respect to the axis Ox which is parallel to the initial polarization. The plane of polarization of the vibration has rotated by an angle α , proportional to the thickness z of crystal traversed, and such that: α =

k0 (nr − nl )z π(nr − nl )z = . 2 λ

388

Symmetry and Physical Properties of Crystals

Here, α positive corresponds to the trigonometric sense, hence to a rotation to the left for an observer with the propagation vector of the incoming light pointing toward her, i.e. for an observer looking at the source: thus the crystal would be levogyre. Taking into account the convention on the sign of rotation deﬁned in the preceding section, α = −α, and the rotatory power ρ = α/z is equal to: π(nl − nr ) . (18.2) ρ= λ The material is dextrogyre if nl > nr , hence if the propagation velocity vr of right-circular polarized waves is larger than the propagation velocity vl of the left-circular polarized waves, and conversely for a levogyre crystal. Dextrogyre quartz has a rotatory power equal to 18.8◦ per mm for wavelength 632.8 nm (red helium-neon laser). Therefore nl − nr = 6.6 × 10−5 , a very small value compared to the birefringence of most crystals, which is on the order of 10−3 . For quartz, ne = 1.5533, no = 1.5442 and ne − no = 9 × 10−3 .

18.3. Interpretation of rotatory power through the inﬂuence of the local environment 18.3.1. Eﬀect of spatial dispersion Until now, we assumed that the electrical polarization at a point depends only on the electric ﬁeld at this point. Actually polarization can also depend on the local environment. This is described by a spatial dispersion term. The relation between E and D was, till now, described (see Eq. (16.22)) as: Em = ηmn

Dn . ε0

(18.3)

To account for spatial dispersion, we must add to Equation (18.3) a term proportional to the space derivatives of induction:

∂Dn 1 ηmn Dn + γmnp . (18.4) Em = ε0 ∂xp We seek a solution in the form of a plane sinusoidal wave: D = D0 exp i(k · r − ωt). We then have:

∂Dn = ikp Dn = iksp Dn ∂xp

where the si are the components of the unit vector parallel to k (k = ks). To simplify notations, we set βmnp = kγmnp , and Equation (18.4) becomes: Em =

1 (ηmn Dn + iβmnp sp Dn ). ε0

(18.5)

Chapter 18 – Rotatory power and optical activity

389

It can be shown [1] that tensor β, called the gyration tensor, is antisymmetric with respect to the ﬁrst two subscripts: βmnp = −βnmp . Among the 27 components βmnp , 9 (those of the form βiil ) are therefore zero, and the remaining 18 (of the form βijl with i = j) are pairwise opposite. There are thus 9 independent components. We deﬁne two-subscript components Gml through: 1 (18.6) Gml = δmij βijl 2 where δmij is the Levi-Civita symbol, or permutation tensor, which was deﬁned in Section 10.6.2 and which is shown to be an axial rank-3 tensor in Section 18A.2. We see for example that: 1 1 G11 = (δ123 β231 + δ132 β321 ) = (β231 − β321 ) or G11 = β231 = −β321 . 2 2 In the same way, G22 = β312 = −β132 ,

G12 = β232 = −β322 ,

etc.

It is easily shown (Sect. 18A.3) that performing a change in frame on the δmij ’s and the βijl ’s transforms the Gml ’s like the components of an axial rank-2 tensor. The axial rank-2 tensor [G] is called the gyrotropy tensor.2 We will see that rotatory power is described by the symmetrical part of [G] alone. Therefore all crystals for which [G] is non zero will be called optically active, whether the symmetrical part is zero or not. Those for which the symmetrical part of [G] is non zero (Sect. 18.5) will be said to feature rotatory power. We will also show (Sect. 18A.4) that relation (18.6) leads to: βijl = δijn Gnl and Equation (18.5) becomes: Em =

1 (ηmn Dn + iδmnj Gjp sp Dn ). ε0

(18.7)

We deﬁne axial vector g through its components gj = Gjp sp and:

g = [G]s.

(18.8)

Equation (18.7) becomes: Em =

1 (ηmn Dn + iδmnj gj Dn ). ε0

2. Some authors call [G] the gyration tensor. Here, we call it the gyrotropy tensor, in order to clearly distinguish it from [β], the gyration tensor (Eq. (18.6)).

390

Symmetry and Physical Properties of Crystals

The second term in the right-hand side is the m-th component of the cross product of vector D with vector g , and we can write: 1 E = ([η]D + iD × g ). (18.9) ε0 Optical activity introduces a purely imaginary term into the impermeability tensor.

We assumed, as in the preceding chapters (see Sect. 16.1), that the crystals are perfectly transparent, i.e. that absorption is zero. If it were not zero, absorption would correspond to a non-zero imaginary part in tensor [η]. The imaginary part which appears here in the relation between D and E has nothing to do with absorption. It introduces between E and D a phase-shift term which, as we will show further on, induces a diﬀerence between the indices of the material for the right- and left-circular polarizations which correspond to the eigenmodes. If absorption were to be taken into account, we would have to consider tensor [β] as complex, and to deal with its imaginary part. A complete treatment taking into account absorption can be found in the books by Agranovich and Ginzburg [2] and Barron [3].

18.3.2. Wave propagation in optically active crystals We saw (Eq. (16.15a)) that the propagation of a sinusoidal electromagnetic wave is described by the basic equation, reproduced here: D = ε0 n2 [E − s(s · E)]

(18.10)

where s is a unit vector parallel to the wave-vector. In Chapter 16, to obtain the propagation behavior of waves in a crystal, we associated to (18.10) relation E = [η]D/ε0 , which we must now replace with Equation (18.9). Since D is perpendicular to s (Eq. (16.10a), a result which is easily retrieved by writing the dot product of D and s in (18.10)), the search for vectors D that are solutions of (18.9) and (18.10) is simpliﬁed by projecting these equations onto a plane perpendicular to s. We choose Ox3 to be parallel to s, and we simplify the form of tensor [η] by choosing for Ox1 and Ox2 the directions of the axes of the ellipse along which the index ellipsoid intersects the plane perpendicular to s. In this coordinate system, tensor [η] can be written as: ⎞ ⎛ 0 η13 η1 ⎝ 0 η2 η23 ⎠ . η13 η23 η33 To simplify the analysis of the general case in what follows, we henceforth choose axis Ox1 such that η1 > η2 . Projecting (18.10) onto Ox1 and Ox2 provides: D1 = ε0 n2 E1 2

D2 = ε0 n E2 .

(18.11a) (18.11b)

Chapter 18 – Rotatory power and optical activity

391

Projecting (18.9) yields: D1 D2 + ig3 (18.12a) ε0 ε0 D2 D1 E2 = η2 − ig3 (18.12b) ε0 ε0 ⎞ ⎛ ⎞ ⎛ ⎞ ⎛ D1 D2 g3 g1 ⎠. −D1 g3 D × g = ⎝ D2 ⎠ × ⎝ g2 ⎠ = ⎝ 0 g3 D1 g2 − D2 g1 E1 = η1

because

Substituting in system (18.12) the values of E1 and E2 by their values as determined from system (18.11), we obtain: D1 D2 1 D1 = η1 + ig3 2 n ε0 ε0 ε0 1 D2 D2 D1 = η2 − ig3 . n2 ε0 ε0 ε0 This system can be written as: D 1 D =M n 2 0 0

with M=

η1 ig3 −ig3 η2

.

The solutions are the eigenvectors of matrix M . The eigenvalues λ of this matrix are the values of 1/n2 . They are obtained by solving equation: (η1 − λ)(η2 − λ) − g32 = 0.

(18.13)

Only the component g3 of g is used. The deﬁnition (18.8) of g makes it possible to write: gj = Gjp sp . Since, in the coordinate system we chose, s = (0, 0, 1), we deduce that g3 = G33 . Here the axis system, which we note R, is associated to the direction of the wave-vector. The gyrotropy tensor is in general deﬁned by its components Gij in an orthonormal axis system R associated to the crystal lattice. Let {aij } be the transformation matrix for going over from the orthonormal axis system R associated to the crystal lattice to the orthonormal axis system R associated to the wave-vector direction. We obtain: G33 = Δa3i a3j Gij = Δsi sj Gij where s1 , s2 and s3 are the components of vector s in the frame R associated to the crystal lattice. The determinant Δ of the transformation matrix is equal to 1 because frames R and R are both chosen to be direct. Finally: g3 = G33 = Gij si sj .

(18.14)

392

Symmetry and Physical Properties of Crystals

A special case: propagation along an optic axis This is the most frequent case in experiments, because then birefringence has no eﬀect, and optical activity is evidenced on its own. If s is parallel to an optic axis, then: 1 (18.15) η1 = η2 = 2 no where no is the index for propagation along the optic axis. For a uniaxial crystal, no is the ordinary index. Equation (18.13) has solutions λ = η1 ± g where, to simplify notations, we note g = g3 . The eigenvectors are then:

1 1 for λ = 2 = η1 + g, which is a right-circular polarized wave; −i n

1 1 for λ = 2 = η1 − g, which is a left-circular polarized wave (Sect. 17.2). i n We retrieve Fresnel’s assumption of two waves, right- and left-circular polarized, propagating with diﬀerent indices, nr and nl . Using (18.15), we obtain:

so that

1 1 1 1 = 2 +g and = 2 −g n2r no no n2l

1 2Δn Δ = − 3 = −2g n2 n

where Δn = nl − nr . We obtain Δn = nl − nr = gn3o and ρ=

π 3 gn λ o

g = Gij si sj ,

with

(18.16) (18.17)

where Gij , si , sj are components in the orthonormal axis system associated to the crystal. General case The eigenvalue Equation (18.13) has solution: λ± =

1 (η1 + η2 ) 1 ± [(η1 − η2 )2 + 4g2 ] 2 . 2 2

We recall that Ox1 was chosen such that η1 > η2 . We deﬁne τ such that: 1

[(η1 − η2 )2 + 4g2 ] 2 − [η1 − η2 ] = τ g, 2

Chapter 18 – Rotatory power and optical activity

393

and we note that |τ | ≤ 1 and τ g > 0. We obtain:

λ+ = η1 + τ g

and

λ− = η2 − τ g.

The associated eigenvectors are respectively:

1 τ and , −iτ i i.e. elliptical vibrations, the axes of which are the directions of the inductions which would propagate in the material if optical activity were neglected. We check that, for propagation along the optic axis, where η1 = η2 , we obtain τ = 1 if g > 0 and τ = −1 if g < 0, and thus right- and left-circular polarizations. Further, if g > 0, nr < nl (since τ = 1) and ρ is positive while, if g < 0, nr > nl and ρ is negative, in agreement with (18.16). As soon as the propagation direction deviates by a few degrees from the direction of the optic axis, η1 − η2 becomes large compared to g. We then ﬁnd τ g/(η1 − η2 ) so that τ 1. The waves have weak ellipticity. The major axes of these vibrations are parallel to the vibrations which would propagate if optical activity were neglected.

18.4. Eﬀect of crystal symmetry on the gyrotropy tensor The axial tensor [G] has no reason to be symmetric. However, (18.17) shows that only the symmetrical part of [G] is involved in rotatory power (18.16). The components of [G] with diﬀerent subscripts combine in (18.17) as, for example, (G12 +G21 )s1 s2 etc. However, it is interesting to begin by considering the whole tensor which represents the total optical activity, keeping in mind that only the symmetrical part of [G] is of interest for the rotatory power.

18.4.1. Centrosymmetric groups The axial rank-2 tensor [G] derives from the polar rank-3 tensor [β]. It is therefore clear that it is identically zero for all centrosymmetric crystal groups. This result can be retrieved directly using axial tensor [G]. The components Gij of an axial rank-2 tensor in an orthonormal coordinate system (Ox1 x2 x3 ) deduced from another orthonormal coordinate system (Ox1 x2 x3 ) through the transformation matrix {aij } are expressed as a function of the components Gij in the coordinate system (Ox1 x2 x3 ) through relation: Gij = Δaim ajn Gmn ,

(18.18)

394

Symmetry and Physical Properties of Crystals

where Δ is the determinant of matrix {aij } (see Eq. (18A.1)). If the crystal is centrosymmetric, a change from referential (Ox1 x2 x3 ) to the referential symmetric with respect to origin O must also leave the components of G unchanged, and Gij = Gij . But in this transformation aij = −δij and Δ = −1. Hence: Gij = −Gij . Finally

Gij = Gij = −Gij

and

Gij = 0.

18.4.2. Non-centrosymmetric groups We now examine some point groups using the direct inspection method. Group 2 We choose Ox3 to be parallel to the 2-fold axis. A rotation by π of the coordinate system (Ox1 x2 x3 ) around the 2-fold axis changes it into system (Ox1 x2 x3 ). The components of a vector transform according to x1 = −x1 ,

x2 = −x2

and x3 = x3 .

For a rotation, Δ = 1, hence [G] has form: 0 0

Group m We choose axis Ox3 perpendicular to the mirror. The operation of symmetry with respect to the mirror, when performed on the axis system, changes the components of a vector according to x1 = x1 ,

x2 = x2

and x3 = −x3 .

For mirror symmetry, Δ = −1, hence [G] has form: 0 0 0 0

Using the preceding result, we immediately see that, if we add to this mirror a 2-fold axis perpendicular to the mirror, hence parallel to Ox3 , all terms in this tensor are zero. This is no surprise since group 2/m is centrosymmetric. We note that the existence of a mirror implies that the trace of the matrix representing [G] is zero.

Chapter 18 – Rotatory power and optical activity

395

Group 4 We choose axis Ox3 parallel to the 4-fold axis. A rotation by π/2 of the coordinate system (Ox1 x2 x3 ) around the 4-fold axis changes it into system (Ox1 x2 x3 ), and the components of a vector transform according to x1 = x2 ,

x2 = −x1

and x3 = x3 .

For a rotation, Δ = 1 and [G] has form 0 0 0 0

where the empty circle connected to the full circle means that the two connected coeﬃcients have equal absolute values and opposite signs. We notice that here G12 = −G21 , so that [G] has an antisymmetric part. Rotatory power depends on the symmetric part of [G], so that the tensor representing the rotatory power has form: 0 0 0 0 0 0

Group 422 Group 422 deduces from group 4 by addition of a two-fold axis perpendicular to the 4-fold axis. One chooses the Ox3 axis parallel to the 4-fold axis and the Ox1 and Ox2 axes parallel to the two-fold axes. A rotation of the coordinate system (Ox1 x2 x3 ) by π around the 2-fold axis parallel to Ox1 changes it into system (Ox1 x2 x3 ), and the components of a vector transform according to x1 = x1 ,

x2 = −x2

and x3 = −x3 .

Δ = 1 and G12 = −G12 = G12 = 0. Tensor [G] is now symmetric and identical to the symmetric part of [G] for point group 4. Group 4mm Group 4mm deduces from group 4 by addition of a mirror parallel to the 4-fold axis. One chooses the Ox3 axis parallel to the 4-fold axis and the Ox1 and Ox2 axes perpendicular to the mirrors. A mirror symmetry normal to Ox1 transforms the coordinate system (Ox1 x2 x3 ) into system (Ox1 x2 x3 ), and the components of a vector transform according to x1 = −x1 ,

x2 = x2

and x3 = x3 .

396

Symmetry and Physical Properties of Crystals

For a mirror symmetry, Δ = −1 and G11 = G22 = G33 = 0 whereas G12 and G21 are not zero. The [G] tensor is now antisymmetric :

( ( 0 0 0 0 0 0

0

so that crystals belonging to class 4mm do not feature rotatory power. Table 18.1 gives the form of the gyrotropy tensor [G] for 18 out of the 21 noncentrosymmetric crystallographic groups. For the three other groups (¯43m, ¯ 62m and ¯6), all components are zero. For three groups (4mm, 3m and 6mm), tensor [G] is antisymmetric: thus they do not feature rotatory power, but they are optically active because of this antisymmetric [G] tensor. We showed (Sect. 10.6) that a rank-2 antisymmetric polar tensor is equivalent to an axial vector. In the same way, it can be shown that a rank-2 antisymmetric axial tensor is equivalent to a polar vector. The gyrotropy tensor of crystal classes 4mm, 3m and 6mm thus has only a vectorial part. It is interesting to note that all the crystal classes for which the [G] tensor involves a vectorial part (1, 2, m, mm2, 4, 4mm, 3, 3m, 6, 6mm) are just the pyroelectric classes. This vectorial part of the gyrotropy tensor can be evidenced using quite delicate reﬂectivity experiments. Table 18.2 gives the form of the symmetric part of the gyrotropy tensor or rotatory power tensor.

18.5. Rotatory power and chirality Table 18.3 gives examples of crystals featuring rotatory power, and the value of their rotatory power ρ (in absolute value) for a given wavelength. Wavelength 632.8 nm is that of the helium-neon laser. The crystals mentioned in this table belong to one of the crystal groups called enantiomorphic or chiral groups. These groups, featuring neither a mirror nor a center of symmetry, and, in a more general way, no roto-inversion, are groups 1, 2, 222, 3, 32, 4, 422, 6, 622, 23, 432. An object is said to be chiral if it is not superimposable with its image in a mirror. This is the case for a hand (in Greek: χειρ, hence the term chiral). The mirror image of a right hand is a left hand. In the same way, a helix is a chiral object: the mirror image of a right-handed helix is a left-handed helix, and conversely. Crystals belonging to these enantiomorphic groups can exist under two forms, called enantiomorphic, one dextrogyre, the other levogyre. Their structures deduce from each other through a mirror symmetry operation. For those whose space group has deﬁnite chirality because it includes a screw axis giving equivalent atom positions located on a right- or left-handed helix (31 and 32 for example),

Chapter 18 – Rotatory power and optical activity

397

Table 18.1: Form of the gyrotropy tensor [G ] Triclinic 1 Monoclinic

2

0 0

2 Ox 3

2 Ox 2

0 0

m

m Ox 3

0 0 0 0

m Ox 2 0

Orthorhombic 222

0 0 0 0 0 0 0 0

Tetragonal 4

Rhombohedral and Hexagonal

0 0 0 0 0 0 0

3, 6 0 0

Cubic 23, 432 Equal components

0

0 0 0

0

mm2

0

0 0 0 0 0 0

422

0 0 0 0 0 0

– 42m 2 Ox1

0 0 0 0 0 0 0

32, 622 2 Ox1

0 0 0 0 0 0

0 0 – 4

0 0

0 0

0

4mm

3m, 6mm m Ox 1

0 0 0 0 0 0

0

0 0 0 0 0 0

0 0 0 0 0 0 Components with equal absolute values but opposite signs

the space groups of crystals of these two enantiomorphic forms are diﬀerent. For example, right-handed quartz has space group P31 21 and left-handed quartz P32 21. The connection between the chirality of the crystal structure and the sign of the rotatory power has long been discussed, and it is no trivial matter. Rotatory power is due to the most polarizable atoms. If these atoms are not in equivalent crystal sites, they can actually form pseudo-helices with chirality opposite to the chirality of the crystal axis, as was shown by A.M. Glazer and K. Stadnicka [4]. The same authors showed that, in crystals where the screw axes have no deﬁnite chirality, such as 63 or 21 (Sect. 7.2.1), the most polarizable atoms form pseudo-helices with given chirality for a given enantiomorph. It can be noticed that the trace of the matrix representing tensor [G] in enantiomorphic classes is non zero whereas for the other crystals featuring rotatory power the trace is zero. This is not surprising since we already noticed that, for crystal classes with a mirror symmetry the trace of [G] is zero (see group m in Sect. 18.4.2).

398

Symmetry and Physical Properties of Crystals

Table 18.2: Form of the symmetrical part of the gyrotropy tensor [G ] for the various point groups. Only the coeﬃcients on the diagonal and in the part above it are represented. Triclinic 1 Monoclinic

0 0

2

2 Ox 3

m

m Ox 3

0 0 0

0

2 Ox 2

m Ox 2

0 0

0 0

0 222

0 0 0

mm2

4, 422

0 0 0

– 4

3, 32, 6, 622

0 0 0

23, 432

0 0 0

Orthorhombic

Tetragonal

Rhombohedral and Hexagonal

0

Cubic

Equal components

0

0 0 0 0 0 0 0

– 42m 2 Ox1

0 0 0 0

Components with equal absolute values but opposite signs

Table 18.3: Values of the rotatory power ρ of some crystals Material

Quartz (SiO2 )

Point group 32

Space group P31 21

Wavelength (nm)

ρ (degree . mm−1 )

643.8

18

274.0

122.1

Berlinite (AlPO4 )

32

P31 21

632.8

14.6

Cinnabar (HgS)

32

P31 21

632.8

320

NaBrO3

23

P21 3

632.8

1.65

NaClO3

23

P21 3

632.8

2.44

α−LiIO3

23

P63 2

632.8

86.7

Chapter 18 – Rotatory power and optical activity

399

While rotatory power is possible for all crystals belonging to an enantiomorphic group, the converse property is not true: belonging to an enantiomorphic group is not a necessary condition for a crystal to feature rotatory power. This is shown on Table 18.2, where non-enantiomorphic groups m, mm2, ¯4 and ¯42m are seen to feature rotatory power. However, the rotatory power of these crystals is often diﬃcult to measure, because they do not necessarily feature rotatory power along the optical axis, and it is then necessary to measure a rotatory power combined with birefringence. The sign of the rotatory power in these crystals depends on the direction of the incident beam, and the crystal is dextrogyre or levogyre depending on this direction. Take the example of a crystal with point group mm2, for which tensor [G] has only one non-zero component, G12 .3 From (18.16) and (18.17), its rotatory power is proportional to G12 s1 s2 . If the optic axes for this crystal are in plane (Ox1 x2 ), the sign of the rotatory power is positive along one of the axes, and negative along the other one, since the product s1 s2 changes sign from one optic axis to the other. This is the case for sodium nitrite NaNO2 in its ferroelectric phase (T < 163◦ C), where rotatory power was measured for wavelength 632.8 nm (Fig. 18.3). Along one of the optic axes, the rotatory power is 15.7◦ /mm, while it has the same value but opposite sign along the other optic axis. M optic axis

optic axis b a

M

Figure 18.3: Plane (a, b), and therefore (Ox 1 , Ox 2 ) for a crystal of sodium nitrite (NaNO2 ). The angle α between the optic axes and one of the two mirrors M is equal to 33◦ . These results are interpreted by taking into account the positions of the ions in the unit cell: they form a left-handed helix along an axis approximately parallel to one of the optic axes, and form a right-handed helix along an axis approximately parallel to the other optic axis. The two optic axes deduce from each other through a mirror operation which changes the right-handed helix into a left-handed helix and vice-versa. In contrast, if the optic axes are in the plane perpendicular to Ox1 or to Ox2 (a frequent case), the rotatory power along the optic axes is zero (s1 or s2 being equal to zero), and the rotatory power becomes very diﬃcult to measure. 3. We recall that, for an orthorhombic crystal with point group mm2, the basis vector c (and thus axis Ox3 ) is chosen parallel to the 2-fold axis.

400

Symmetry and Physical Properties of Crystals

18.6. Absorption and conclusion We neglected absorption, which is extremely weak in transparent crystals at the wavelengths in the visible range considered here. We thus neglected the imaginary part of the index. The real and imaginary parts of the index are not independent. They are connected through integral relations (involving integration over the whole frequency range) known as the Kramers-Kronig relations (see [5]). As a consequence, a diﬀerence in index for two diﬀerent polarizations leads to a notable diﬀerence in absorption near an absorption edge: this is dichroism. The birefringence discussed in Chapter 16 corresponds to a difference in index for two orthogonal linear polarizations. There is therefore a diﬀerence in absorption for these two polarizations, hence linear dichroism. The rotatory power is due to a diﬀerence in index for the right-circular and left-circular polarizations, which leads to a diﬀerence in absorption for these two polarizations, hence circular dichroism. In the X-ray range, where crystals are not transparent, optical activity was experimentally evidenced recently, through dichroism measurements for natural rotatory power [6], and through reﬂectivity measurements for the vectorial part of [G] [7]. We showed that, among the 21 non-centrosymmetric crystal classes, 18 are optically active. Out of these 18 classes, 15 feature rotatory power. Among these 15 classes, 11 are enantiomorphic, which means that crystals in these classes can exist under two diﬀerent, mutually symmetric forms, one dextrogyre and the other levogyre. We have seen that the gyrotropic tensor of enantiomorphic classes has non-zero trace whereas, for the 4 non-enantiomorphic classes, the trace of [G] is zero. For the 3 optically active classes which do not feature rotatory power, the axial tensor [G] is antisymmetric and can be represented by a vector. This distinction between enantiomorphic crystals, non-enantiomorphic crystals which nevertheless feature rotatory power, and optically active crystals just on the basis of the vector part of [G], was ﬁrst introduced by Jerphagnon and Chemla in 1976 [8]. These authors split the symmetric part of [G] into the sum of an isotropic tensor (proportional to the unit tensor), which they note [A], and a tensor [D]. Thus the gyrotropy tensor [G] is the sum of [A], [D] and the vector part V (equivalent to the antisymmetric part of [G]). For enantiomorphic crystals, [A] is not zero, all crystals featuring rotatory power have [A] + [D] non zero, and optically active crystals with no rotatory power have only V non zero.

Chapter 18 – Rotatory power and optical activity

401

Complement 18C. Magnetic optical rotation The magneto-optical eﬀects can be deﬁned as the eﬀects of a magnetic ﬁeld on the propagation of an electro-magnetic wave, and can be described through the change in the high-frequency susceptibility tensor and refractive indices of a material due to the magnetic ﬁeld. The Faraday magneto-optical eﬀect, or magnetic gyrotropy, is the best-known member of this family. It concerns visible and near-visible light, but is now also an active ﬁeld of research, using synchrotron radiation, in the X-ray spectral range. The Faraday eﬀect, discovered in 1845, consists in the rotation4 of the plane of polarization of linearly polarized light under the inﬂuence of a magnetic ﬁeld B or magnetization parallel to the propagation direction. It is thus reminiscent of natural rotatory power, discussed in this chapter. It too can be conveniently described through the diﬀerence in the refractive indices, hence the diﬀerent phase velocities, associated to the right- and left-hand circular polarization states which are the eigenmodes. In materials with no spontaneous magnetization, such as dia- or paramagnets, the rotation α is proportional to the modulus of the magnetic ﬁeld B and to the length of material d traversed by the light beam: α = kV Bd,

where kV is the Verdet “constant”, a material-dependent function of the temperature and wavelength, with values on the order of 101 rad T−1 m−1 . In materials with spontaneous magnetization, typically ferrimagnets which are fairly transparent in the visible and near infra-red range, the eﬀect of the magnetic ﬁeld is primarily to steer the distribution of local magnetization in the various domains (see note in Complement 8C), favoring those with direction close to the ﬁeld, and tending toward saturation. The rotation is then α = θF d, with θF the rotation per unit length for magnetization parallel to the magnetic ﬁeld. Values are on the order of 104 degree cm−1 for substituted iron garnets (BiRGa)Fe5 O12 where R is a rare-earth element. An essential feature that distinguishes magnetic and natural rotatory power is the behavior under reversal of the propagation direction of light. After two successive passes in opposite directions through a sample, the eﬀect of spontaneous rotatory power cancels out. In the case of magneto-optical activity, in contrast, the rotation of the plane of polarization is doubled (Fig. 18C.1). This is usually designated as non-reciprocity, and is related to the non-invariance under time reversal (see Complement 8C) featured by a system with magnetization.

4. The rotation is actually complemented by the appearance of ellipticity.

402

Symmetry and Physical Properties of Crystals E0

B

E1

B E2

(a)

E1

(b)

Figure 18C.1: (a) Faraday rotation in an isotropic material (for example

a liquid) submitted to magnetic ﬁeld B: the polarization of the light is rotated by the angle α between E0 and E1 ; it is here counterclockwise as seen by an observer looking at the light source. With just the magnetic ﬁeld reversed, the rotation of the polarization becomes −α, clockwise for the observer. (b) The propagation direction is reversed, but not the magnetic ﬁeld: the rotation of the polarization is now clockwise for the observer (looking at the source, hence to the right), and therefore counterclockwise when looking along the propagation direction. Hence the overall rotation with respect to the laboratory frame, after two passes in opposite directions, is 2α. The Faraday eﬀect in ferrimagnets has applications such as magneto-optical isolators (preventing light from propagating in one direction), magnetic ﬁeld sensors, or the observation of magnetic domains and of magnetic ﬁeld maps.

Further reading E. du Trémolet de Lacheisserie, D. Gignoux and M. Schlenker (ed.), Magnetism, vol. 1: Fundamentals (Springer Verlag, New York and Heidelberg, 2005), chap. 13

Chapter 18 – Rotatory power and optical activity

403

Appendix 18A. Axial tensors, or pseudo-tensors 18A.1. Deﬁnition of axial tensors, or pseudo-tensors In Chapter 9, we deﬁned a rank-n tensor as a mathematical object having, in a given orthonormal frame, 3n components (if considering three-dimensional space) which, in a change of orthonormal frame, transform like the product of n components of vectors. This deﬁnition corresponds to polar tensors. Consider for example a rank-3 tensor, with components Tijk in a given frame. After a change in frame characterized by transformation matrix A, with coeﬃcients aij , such that: the new components of this tensor become Tmnp Tmnp = ami anj apk Tijk .

A polar vector is a rank-1 tensor. We saw (Eq. (10.13)) that the components wi of an axial vector, or pseudo such that: vector, transform in a change of orthonormal frame into wm = Δami wi wm

where Δ is the determinant of the transformation matrix, +1 for direct (or proper) transformations, and −1 for indirect (or improper) transformations. More generally, pseudo-tensors (or axial tensors) of rank n are deﬁned as mathematical objects having, in a given orthonormal frame, 3n components which, in a change of frame, transform like the product of n components, multiplied by the determinant of the matrix transforming one frame into the other. For example, a rank-3 axial tensor with components Vijk in a given frame will, in another frame deduced from the previous one through the transformation such that: matrix A, have components Vmnp = Δami anj apk Vijk . Vmnp

(18A.1)

18A.2. Levi-Civita tensor, or permutation tensor In Section 10.6.2, we deﬁned the Levi-Civita symbol, δijk , such that, whatever the coordinate system used, δijk = 0 if at least two of the subscripts i, j and k are equal, δijk = 1 if the permutation ijk is direct (123, 231, 312), δijk = −1 if it is indirect (132, 213, 321). To show that this symbol is an axial tensor, we consider ﬁrst the polar tensor of rank 3, εijk , deﬁned in a given system of axes, with basis vectors e1 , e2 and e3 through: εijk = 0 if two of the subscripts i, j or k are equal, εijk = 1 if the circular permutation ijk is direct (123, 231, 312),

404

Symmetry and Physical Properties of Crystals εijk = −1 if it is indirect (132, 213, 321).

In another orthonormal axis system, with basis vectors e1 , e2 and e3 , with transformation matrix {aij }, these components become: εmnp = ami anj apk εijk = am1 (an2 ap3 − an3 ap2 ) + am2 (an3 ap1 − an1 ap3 ) + am3 (an1 ap2 − an2 ap1 ) = [am1 (en × ep )1 + am2 (en × ep )2 + am3 (en × ep )3 ] = em · (en × ep ) = (em , en , ep ).

We thus see that: εmnp = 0 if two of the subscript m, n, p are equal, εmnp = Δ for mnp = 123, 231 and 312, εmnp = −Δ for mnp = 132, 213 and 321, where Δ is the determinant of the transformation matrix. This result shows that the Levi-Civita symbol, which retains the same value irrespective of coordinate changes, must therefore transform in a change of coordinate system in the following way: = Δami anj apk δijk . δmnp

It is therefore a rank-3 pseudo-tensor, or axial tensor, called the permutation tensor.

18A.3. The gyrotropy tensor [G] is a rank-2 axial tensor We show that the gyration tensor Gml is a rank-2 axial tensor by investigating how it transforms in a coordinate system change with transformation matrix {aij }. By deﬁnition (18.6), 1 Gml = δmij βijl 2 where δmij is the permutation tensor, a rank-3 axial tensor, and βijl a polar rank-3 tensor. The new components Guv are such that: Guv =

1 1 δ β = Δaum ain ajp δmnp aik ajl avw βklw . 2 uij ijv 2

From Equation (9.10), ain aik = δnk and ajp ajl = δpl , hence we can write: 1 1 Guv = Δδnk δpl aum avw δmnp βklw = Δaum avw δmnp βnpw = Δaum avw Gmw . 2 2 This shows that [G] is a rank-2 axial tensor.

Chapter 18 – Rotatory power and optical activity

405

18A.4. Relation between tensors [G] and [β] We calculate the product δijn Gnl by using the deﬁnition (18.6) of Gnl . δijn Gnl =

1 δijn δnmp βmpl . 2

For given i, j and n such that δijn = 0, the only non-zero products δijn δnmp are δijn δnij equal to 1, and δijn δnji equal to −1. Hence: δijn Gnl =

1 (βijl − βjil ) = βijl . 2

We obtain the relation: βijl = δijn Gnl .

406

Symmetry and Physical Properties of Crystals

References [1] L.D. Landau, E.M. Lifshitz and L.P. Pitaevskii, Course of Theoretical Physics, vol. 8, Electrodynamics of Continuous Media, 2nd edn. (Elsevier, Oxford, 1984) [2] V.M. Agranovich and V.L. Ginzburg, Crystal Optics with Spatial Dispersion, and Excitons, 2nd edn. (Springer-Verlag, 1984) [3] L. Barron, Molecular Light Scattering and Optical Activity, 2nd edn. (Cambridge University Press, 2004) [4] A.M. Glazer and K. Stadnicka, J. Appl. Cryst. 19, 108–122 (1986) [5] J.D. Jackson, Classical Electrodynamics, 3rd edn. (Wiley, 1998) [6] J. Goulon et al., X-ray natural circular dichroism in uniaxial gyrotropic single crystals of LiIO3 , J. Chem. Phys. 108, 6394–6403 (1998) [7] J. Goulon et al., Vector part of optical activity probed with X-rays in hexagonal ZnO, J. Phys. Condens. Matter 19, 156201–156219 (2007) [8] J. Jerphagnon and D.S. Chemla, J. Chem. Phys. 65, 1522–1529 (1976)

Optical activity in crystals,

Chapter 19

Electro-optical and elasto-optical eﬀects This chapter introduces various eﬀects through which the refractive index of a crystal (directly related to its permittivity tensor) can be altered through an external ﬁeld, such as a static electric ﬁeld or a strain. These changes to the index induced by an external, freely tailored ﬁeld, have many applications. Some of these are introduced as the various eﬀects are discussed.

19.1. Introduction We saw that the optical properties of a crystalline material are directly related to the tensor of electrical impermeability [η]. This tensor is the inverse of the permittivity tensor [ε], which is related to the electrical susceptibility tensor [χ] by relation: [ε] = ε0 ([E] + [χ]) where [E] is the identity tensor. The electrical susceptibility [χ] describes the appearance of a polarization P (electric dipole moment per unit volume) under the action of the electric ﬁeld E of the optical wave incident on the crystal. In Chapter 16, which deals with crystal birefringence, we restricted the Maclaurin expansion of the polarization P of the material as a function of the electric ﬁeld E with angular frequency ω, to the linear term: P(ω) = ε0 [χ]E(ω).

(19.1)

We then showed (Chap. 18) that optical activity is due to the inﬂuence of the local environment on the susceptibility, leading, in the expansion of P as a function of E, to an additional term, proportional to the spatial derivatives of the components of the electric ﬁeld: ∂Ej (ω) Pi (ω) = χij Ej (ω) + χijk . ε0 ∂xk © Springer Science+Business Media Dordrecht 2014 C. Malgrange et al., Symmetry and Physical Properties of Crystals, DOI 10.1007/978-94-017-8993-6_19

(19.2)

407

408

Symmetry and Physical Properties of Crystals

The susceptibility can also be inﬂuenced by the application of a static electric ﬁeld Es which contributes to the expansion (19.2) an additional term of the form χijk Ejs Ek (ω): ∂Ek (ω) Pi (ω) = χij Ej (ω) + χijk + χijk Ejs Ek (ω) + . . . ε0 ∂xj

(19.3)

The expansion can be continued by adding a term depending on the square of the applied static electric ﬁeld, and possibly other terms related to the inﬂuence on the susceptibility of other sorts of applied ﬁelds, such as a strain or a stress or a static magnetic ﬁeld. The existence of these additional terms in the expansion of the susceptibility leads to a dependence of the impermeability tensor [η] on these external applied ﬁelds. This means that optical propagation is coupled, for example, with an applied electric ﬁeld (electro-optical eﬀects), a strain or stress (elasto-optical eﬀects), or a magnetic ﬁeld (magneto-optical eﬀects). These couplings make it possible to alter optical propagation in crystals through these external ﬁelds, and they give rise to many applications. We restrict discussion to a few examples which give insight on how to deal with these couplings. Section 19.2 introduces electro-optical eﬀects, and Section 19.3 introduces elasto-optical eﬀects, which are also called acousto-optical eﬀects when the deformation results from the application of an acoustic wave.

19.2. Electro-optical eﬀects Applying a static electric ﬁeld Es to a crystal alters the dielectric impermeability tensor [η]. We can write: ηij (E) − ηij (E = 0) = Δηij = rijk Ek + zijkl Ek El + . . . To simplify notations, we replaced in this expression Es by E, because there is no ambiguity with the electric ﬁeld E(ω) of the optical wave, since E(ω) is not involved in this expression for [η]. The second-order term is much smaller than the ﬁrst-order one. Therefore we investigate the linear term ﬁrst. The quadratic term is evidenced when the linear term is zero. The coeﬃcients rijk are the components of a rank-3 tensor since they relate rank-1 tensor E with rank-2 tensor [η]. In the same way, coeﬃcients zijkl are the components of a rank-4 tensor.

19.2.1. Linear electro-optical eﬀect, or Pockels eﬀect General properties The changes induced on the tensor by a static electric ﬁeld E are small, even for rather strong applied ﬁelds (104 V cm−1 ). They are of interest only when they bring about a qualitative change to tensor [η]: for instance when a cubic,

Chapter 19 – Electro-optical and elasto-optical eﬀects

409

therefore optically isotropic, crystal becomes optically anisotropic (induced birefringence), or when a uniaxial crystal becomes biaxial. This change then has the advantage that it can be modulated by altering the amplitude of the electric ﬁeld. The linear eﬀect is described by: Δηij = rijk Ek where the rijk are the coeﬃcients of the electro-optical Pockels rank-3 tensor, [r]. Tensor [Δη], the diﬀerence between two symmetric tensors, is symmetric, and the two-subscript notation involving i and j can be replaced by a singlesubscript notation, as was done for the stress tensor [T ]. We then obtain six components Δηα , where α ranges from 1 to 6, and tensor rijk can be written with two subscripts. We note that, in contrast to the piezoelectric tensor (Sect. 15.3.2), no doubling occurs when going over from the rijk to the rαk . We have Δη23 = r23k Ek and Δη32 = r32k Ek , and the symmetry of [Δη] leads to r23k = r32k . We can write:

Δη4 = Δη23 = Δη32 = r4k Ek

with r4k = r23k = r32k , so that: Δηα = rαk Ek . In matrix notation, the vectors with components Δηα and Ek are column vectors, and the components rαk form a matrix with 6 rows and 3 columns, as for the inverse piezoelectric eﬀect. ⎞ ⎛ ⎞ ⎛ Δη1 r11 r12 r13 ⎜ Δη2 ⎟ ⎜ r21 r22 r23 ⎟ ⎛ ⎞ ⎟ ⎜ ⎟ ⎜ E1 ⎜ Δη3 ⎟ ⎜ r31 r32 r33 ⎟ ⎟ ⎜ ⎟ ⎝ E2 ⎠ . ⎜ ⎜ Δη4 ⎟ = ⎜ r41 r42 r43 ⎟ ⎟ ⎜ ⎟ ⎜ E3 ⎝ Δη5 ⎠ ⎝ r51 r52 r53 ⎠ Δη6 r61 r62 r63 The eﬀect of crystal symmetry on the number of independent components is the same as for the piezoelectric tensor. We therefore refer to Table 15.2, using the transposed matrices (Tab. 19.1a and 19.1b) and taking into account the fact that rαk = rijk for α = 4, 5, 6 whereas diα = 2dijk . We recall that material rank-3 tensors are zero for all centrosymmetric crystals. The order of magnitude of the non-zero components of tensor [r] is 10−12 m V−1 , thus picometres per volt (pm V−1 ).

410

Symmetry and Physical Properties of Crystals

Table 19.1a : Form of the matrices representing the electro-optical Pockels tensor (linear eﬀect) for various point groups 1

Triclinic

Monoclinic

2 2 Ox2

0 0 0

m 2 Ox3

0 0

0 0 0 0

0

0 0

0 0

Orthorhombic

Tetragonal

0 0

0 0

0 0

0

0 0

0

0

222

mm2

0 0 0 0 0 0 0 0 0 0 0 0 0 0 0

0 0 0 0 0 0 0 0 0 0 0 0 0

4

– 4

422

4mm

0 0 0 0 0 0 0 0 0 0 0

0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0

0 0 0 0 0 0 0 0 0 0 0 0 0

0 0 0 0 0 0 0 0 0 0 0

m Ox3

0 0 0 0

0 0

m Ox2

Equal components Components with equal absolute values but opposite signs

0 0 0 0 0

– 42m (2 Ox1)

0 0 0 0 0 0 0 0 0 0 0 0 0 0 0

Chapter 19 – Electro-optical and elasto-optical eﬀects

411

Table 19.1b : Form of the matrices representing the electro-optical Pockels tensor (linear eﬀect) for various point groups (continued) 3

Rhombohedral

32

3m

2 Ox1

0 0 0 0 0 0 0 0 0

0 0 0 0 0 Hexagonal

6

0 0 0 0 0 0 0 0 0 0 0

0 0 0 0

m Ox1

0 0

0 0 0 0 0 0 0 0

– 6

622

0 0 0 0 0 0 0 0 0 0 0 0

0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0

– 62m m Ox2

0 0 0 0 0 0 0 0 0 0

0 0 0 0 0 0

0 0 0 0

0 0 0 0 0 0 0 0

0 0 0 0 0

0 0 0 0 0

0 0 0 0 0

432

– 43m, 23

0 0 0 0 0 0

0 0 0 0 0 0

0 0 0 0 0 0

0 0 0 0 0 0 0 0

6mm

m Ox1

Cubic

m Ox2

0 0

0 0 0 0 0 0 0 0 0 0 0 0 0 0 0

Equal components Components with equal absolute values but opposite signs

412

Symmetry and Physical Properties of Crystals

Example of a cubic crystal with point group 23 This corresponds to crystals of sodium bromate NaBrO3 or of sodium chlorate NaClO3 . Tensor [r], expressed in the crystallographic axis system, has only three nonzero components which are equal to one another, r41 = r52 = r63 . Consider a crystal plate of NaBrO3 (or NaClO3 ), with faces perpendicular to one of the 2-fold axes, chosen as Ox3 . We apply an electric ﬁeld perpendicular to the plate (Fig. 19.1a). n + r41 En3/2

x2 b

k

n – r41 En3/2

x’2

x1 a c

x2

x’1 b

x3

O

a

x1

E

(a)

(b)

Figure 19.1: (a) Schematic representation of optical propagation in a crystal of NaClO3 submitted to an electric ﬁeld parallel to basis vector c; (b) directions of the neutral lines of the plate (dotted lines) We have: ⎛ ⎜ ⎜ ⎜ ⎜ ⎜ ⎜ ⎝

Δη1 Δη2 Δη3 Δη4 Δη5 Δη6

⎞

⎛

⎟ ⎜ ⎟ ⎜ ⎟ ⎜ ⎟=⎜ ⎟ ⎜ ⎟ ⎜ ⎠ ⎝

0 0 0 0 0 0 0 0 0 0 r41 0 0 r41 0 0 0 r41

⎞

⎛

⎟⎛ ⎞ ⎜ ⎟ ⎜ 0 ⎟ ⎜ ⎟⎝ 0 ⎠ = ⎜ ⎟ ⎜ ⎟ E ⎜ ⎠ ⎝

0 0 0 0 0 r41 E

⎞ ⎟ ⎟ ⎟ ⎟. ⎟ ⎟ ⎠

[Δη] has one non-zero component, and the electrical impermeability tensor [η] becomes: ⎞ ⎛ r41 E 0 η0 ⎝ r41 E η0 0 ⎠ 0 0 η0 where η0 is the value for zero electric ﬁeld, η0 = 1/n2 (Eq. (16.24)), where n is the index of the crystal without electric ﬁeld. The crystal is now birefringent. Axis Ox3 , parallel to one of the basis vectors of the cubic unit cell of the crystal (c on Fig. 19.1a) and to the applied electric ﬁeld, is a principal axis of the tensor. In an axis system (Ox1 x2 x3 ) rotated by 45◦ around axis Ox3 ,

Chapter 19 – Electro-optical and elasto-optical eﬀects tensor [η] becomes:

⎞

⎛

1 ⎜ n2 + r41 E ⎜ ⎜ 0 ⎜ ⎝ 0

413

0 1 − r41 E n2 0

0 ⎟ ⎟ 0 ⎟ ⎟. 1 ⎠ n2

Axes Ox1 and Ox2 are principal axes. The principal values of tensor [η] are the reciprocals of the squares of the indices ni which deﬁne the index ellipsoid (16.24), hence: 1 1 = 2 + r41 E 2 n n1

and

1 1 = 2 − r41 E. 2 n n2

Suppose we send onto the crystal a plane electromagnetic wave with wavevector k perpendicular to the plate, hence parallel to the electric ﬁeld (Fig. 19.1a). The components of the electric ﬁeld of the wave along Ox1 and Ox2 propagate with diﬀerent indices n1 and n2 (Fig. 19.1b). The diﬀerence Δn = n2 − n1 is easily calculated, because the change induced by the electric ﬁeld is very small. We obtain:

1 Δn (19.4) Δ = −2 3 = −2r41 E n2 n whence we deduce:

Δn = n2 − n1 = n3 r41 E.

The crystal plate has become birefringent, and its birefringence is proportional to the value of the applied electric ﬁeld. Its neutral lines are parallel to Ox1 and Ox2 , thus at 45◦ to vectors a and b. Example of a tetragonal crystal with point group ¯ 42m: a crystal of KDP (potassium dihydrogen phosphate KH2 PO4 ) We consider a plate of KDP in which the faces are perpendicular to the optic axis (¯4 axis parallel to c), and an incident wave normal to the plate (Fig. 19.2a), thus with wave-vector parallel to the optic axis. When no electric ﬁeld is applied, the plate is isotropic for the incident ray. The electro-optical tensor rijk for point group ¯42m has the form given below in Equation (19.5) if axis Ox3 is chosen parallel to the ¯4 axis and axes Ox1 and Ox2 are parallel to the 2-fold axes. The latter are parallel to basis vectors a and b because the space group of KDP is I¯42d (Sect. 7.4). Suppose we apply an electric ﬁeld, with norm E, parallel to the optic axis, i.e. to the ¯4 axis. Tensor Δηα is such that: ⎞ ⎛ ⎞ ⎛ ⎞ ⎛ Δη1 0 0 0 0 ⎜ Δη2 ⎟ ⎜ 0 ⎛ ⎞ ⎜ 0 ⎟ 0 0 ⎟ ⎟ ⎜ ⎟ ⎜ ⎟ ⎜ 0 ⎟ ⎜ Δη3 ⎟ ⎜ 0 ⎟ ⎜ 0 0 ⎜ ⎟=⎜ ⎟⎝ 0 ⎠ = ⎜ 0 ⎟. (19.5) ⎜ Δη4 ⎟ ⎜ r41 0 ⎟ ⎜ 0 ⎟ 0 ⎟ ⎜ ⎟ ⎜ ⎟ ⎜ E ⎝ Δη5 ⎠ ⎝ 0 r41 0 ⎠ ⎝ 0 ⎠ Δη6

0

0

r63

r63 E

414

Symmetry and Physical Properties of Crystals n + r63 En3/2

x2 b

k

n – r63 En3/2

x’2

x1 a c

x2

x’1 b

x3

O

a

x1

E

(a)

(b)

Figure 19.2: (a) Schematic representation of optical propagation in a crystal of KDP submitted to an electric ﬁeld E parallel to basis vector c; (b) directions of the neutral lines of the plate (dotted lines) We obtain Δη6 = r63 E and all the other terms are zero. Tensor [η] is now given by: ⎞

⎛

1 r63 E ⎜ n2o ⎜ 1 ⎜ r E ⎜ 63 n2o ⎜ ⎝ 0 0

0

⎟ ⎟ 0 ⎟ ⎟ ⎟ 1 ⎠ n2e

where no and ne are respectively the ordinary and extraordinary indices of the KDP crystal without applied electric ﬁeld. Rotation of the axis system by 45◦ around the optic axis Ox3 makes the tensor diagonal: ⎞

⎛

1 + r63 E ⎜ n2o ⎜ ⎜ 0 ⎜ ⎜ ⎝ 0

0 1 − r63 E n2o 0

⎛ 1 ⎟ ⎜ n21 ⎟ ⎜ ⎜ 0 ⎟ ⎟=⎜ 0 ⎟ ⎜ 1 ⎠ ⎝ 0 n2e 0

⎞ 0 1 n22 0

0

⎟ ⎟ 0 ⎟ ⎟ ⎟ 1 ⎠ n23

where n1 , n2 and n3 are the principal indices. The index ellipsoid is no more an ellipsoid of revolution around Ox3 . Its principal axes are Ox3 and two axes Ox1 and Ox2 at 45◦ to the axes Ox1 and Ox2 . Ox1 and Ox2 are thus parallel to the mirrors in the crystal. We have: 1 1 = 2 + r63 E no n21

and

1 1 = 2 − r63 E no n22

Chapter 19 – Electro-optical and elasto-optical eﬀects

415

whence we deduce as above, setting Δn = n2 − n1 :

Δn 1 = −2 3 = −2r63 E, Δ n2 no Δn = n2 − n1 = n3o r63 E.

(19.6)

The neutral lines of the plate are at 45◦ to axes a and b (Fig. 19.2b).

19.2.2. Applications of the linear electro-optical eﬀect Phase-shifting plates with variable delay In the two special cases we discussed previously, applying an electric ﬁeld normal to the plate changes isotropic propagation into anisotropic propagation. The neutral lines of the plate are at 45◦ to the vectors a and b parallel to the plane of the plate. The diﬀerence between the indices for waves with polarization parallel to these neutral lines is proportional to the amplitude E of the electric ﬁeld and to an electro-optical coeﬃcient r (r14 for NaBrO3 and r63 for KDP): Δn = n3 rE. If the beam traverses a thickness e of crystal, the components of the electric ﬁeld of the wave, parallel to the neutral lines of the plate, feature, when leaving the plate, a phase diﬀerence ϕ: ϕ = 2π

n3 rEe n3 rV (Δn)e = 2π = 2π λ λ λ

(19.7)

where V is the voltage applied between the two faces of the crystal. The half-wave voltage Vπ is deﬁned as the voltage which must be applied to the crystal for the phase shift to be equal to π. It is obtained from Equation (19.6), yielding: λ (19.8) Vπ = 3 . 2n r The phase shift can then be written as: ϕ=

πV . Vπ

For a crystal of KDP, r = r63 = 10.3 pm V−1 , n = 1.51 for λ = 545 nm and Vπ = 7.8 kV. For a crystal of NaClO3 , the half-wave voltage, for the same wavelength, is equal to 200 kV. The same plates become quarter-wave plates (ϕ = π/2) if they are submitted to a voltage equal to half the half-wave voltage. We note that the value of the phase shift does not depend on the crystal thickness, but on the voltage applied between its two faces. Thus, in principle, thin crystals can be used. However, since the voltages are rather large, the crystal must be thick enough to avoid electrical breakdown.

416

Symmetry and Physical Properties of Crystals

Longitudinal ﬁeld intensity modulator Consider a crystal of KDP cut into a rectangle parallelepiped with sides parallel to the basis vectors a, b and c of the unit cell (Fig. 19.3). We choose an orthonormal coordinate system (Ox1 x2 x3 ) (the unit vectors on these axes are written as i, j and k) parallel to the basis vectors, and an axis system (Ox1 x2 x3 ) (with unit vectors i , j and k) rotated with respect to the ﬁrst one by 45◦ around Ox3 . A

x2 x1 a P

b c

x3

x2 x’2

x’1 j’

j O

i’ i

x1

L V

Figure 19.3: Intensity modulator with longitudinal ﬁeld We send onto this crystal a plane wave, with wave-vector ko parallel to Ox3 , linearly polarized along Ox2 thanks to a polarizer P. The crystal has length L along the propagation direction. Using transparent electrodes deposited on the entrance and exit surfaces of the crystal, we apply a voltage V , which creates in the crystal an electric ﬁeld E = V /L perpendicular to the plate. The electric ﬁeld of the wave incident on the entrance face of the crystal has form E0 (exp −iωt)j, the origin of the axes being chosen on the entrance face of the crystal. We saw (Sect. 19.2.1) that the neutral lines of the crystal are parallel to Ox1 and Ox2 . The incident polarization √ splits into two components parallel to the √ neutral lines (( 2/2) E0 i and ( 2/2) E0 j ), which propagate with diﬀerent indices and thus shift their phase as propagation proceeds. At the crystal exit, the electric ﬁeld of the wave can be written: √ √ 2 2 E = E0 exp i(k0 n1 L − ωt) i + E0 exp i(k0 n2 L − ωt) j (19.9) 2 2 with

n1 = no −

n3o r63 E , 2

n2 = no +

We set

k0 (n2 − n1 )L = 2δ =

so that

δ=

n3o r63 E 2

and

2π 3 2π 3 n r63 EL = n r63 V λ o λ o

π 3 n r63 V λ o

which only depends on the voltage V applied to the crystal.

k0 =

2π . λ

Chapter 19 – Electro-optical and elasto-optical eﬀects Equation (19.8) can be written as: √ 2 exp i(k0 n1 L − ωt)(i + exp 2iδj ), E = E0 2

417

(19.10)

and, in Jones notation, the electric ﬁeld has expression, in base {i , j }: " # √ 2 E 0 2 √ . E0 22 exp 2iδ We see that, depending on the value 2δ of the phase shift between the two components, the wave can take on, at the crystal exit, any polarization (see Sect. 17.1.3). The crystal is a half-wave plate if the applied voltage Vπ is such that 2δ = π, hence Vπ = λ/2n3 r63 , a value we already found in (19.7). We can thus write that 2δ = πV /Vπ . The electric ﬁeld (19.9) can also be written, to within a phase factor: √ 2 −iδ [E i + E iδ j ]. E = E0 2 A linear analyzer A, with polarization axis parallel to Ox1 , is placed after the crystal (Fig. 19.3). The crystal is thus set between crossed polarizers. The electric ﬁeld after the analyzer is the√sum of the projections onto Ox√ 1 of E. The projection of vector i is vector ( 2/2)i and that of vector j is −( 2/2)i. We obtain an electric ﬁeld E such that E0 −iδ E = − E iδ ]i [E 2 = −iE0 sin δ i. The transmitted intensity I is proportional to the square of the amplitude of the electric ﬁeld (Sect. 16.3), so that:

π V I = I0 sin2 δ = I0 sin2 2Vπ where we note I0 the intensity incident on the crystal. If we apply a voltage equal to Vπ , the intensity is maximum and equal to the intensity transmitted by the polarizer, whereas at zero voltage the intensity is zero (isotropic propagation, crystal placed between crossed polarizer and analyzer). This device can then be used as a beam switch, by changing from voltage Vπ (I = I0 ) to zero voltage (I = 0). If a DC voltage equal to Vπ /2 is sinusoidally modulated with amplitude much smaller than Vπ , the intensity of the light beam is modulated quasi-sinusoidally. The slope of the function I(V ) is nearly constant in the vicinity of Vπ /2 (Fig. 19.4), so that the relation between the voltage variation and the variation in transmitted intensity is quasi-linear. In this setup, the voltage Vπ does not depend on the crystal length; it can therefore not be optimized. Also it is not easy to make transparent electrodes. The setup described next, with transverse ﬁeld, is therefore preferred.

418

Symmetry and Physical Properties of Crystals I/I0 1

V(t)/V

I(t)/I0

0

V/V

1

Figure 19.4: Analog modulation, using the experimental device schematically shown on Figure 19.3 Transverse ﬁeld intensity modulator The crystal used is again a rectangle parallelepiped of KDP, but cut so that its sides are parallel to Ox3 , Ox1 and Ox2 , with the incident beam parallel to Ox1 (Fig. 19.5). It is placed between crossed polarizer and analyzer, the polarization direction of the analyzer being at an angle of 45◦ to the sides of the entrance face of the crystal. The electric ﬁeld is parallel to Ox3 . A

x3 x’2 P

c

b

x’1

a

45°

x3

45°

n

V

k O

L

m j’

x’2

Figure 19.5: Intensity modulator with transverse ﬁeld The neutral lines of the plate are Ox3 and Ox2 , and only the index for the component parallel to Ox2 is modulated by the electric ﬁeld. We note that, in the absence of the electric ﬁeld, the crystal is birefringent for the chosen propagation direction. On the entrance face of the plate, the electric ﬁeld of the light wave can be written as: √ 2 (j + k) exp(− iωt) E = E0 2 taking the origin on the entrance face of the crystal.

Chapter 19 – Electro-optical and elasto-optical eﬀects

419

After the plate, the electric ﬁeld becomes: √

2 1 3 j exp ik0 L no + no r63 E + k exp ik0 Lne exp(−iωt). E = E0 2 2 We set:

1 k0 L(ne − no − n3o r63 E) = 2δ 2 and the electric ﬁeld becomes: √

1 3 2 exp ik0 L no + no r63 E [j + exp 2iδ k] exp(−iωt) E = E0 2 2 and, in Jones notation in base {j , k} : " # " # √ √ 2 2 E E exp −iδ 0 0 2 2√ √ or . E0 22 exp 2iδ E0 22 exp iδ We can thus write the electric ﬁeld, to within a phase factor: √ 2 E = E0 (exp −i δ j + exp i δ k). 2 After the analyzer, the electric ﬁeld E is the projection of E on the unit vector n parallel to the analyzer (Fig. 19.5): E =

E0 [− exp −iδ + exp iδ]n = i(E0 sin δ)n 2

and the intensity I of the light beam is:

1 V πL ne − no − n3o r63 I = I0 sin2 δ = I0 sin2 λ 2 where is the thickness of the crystal in the direction of Ox3 and V the applied voltage (E = V /). We see that the voltage Vπ which changes the phase shift 2δ by π can be strongly decreased if the crystal specimen is long and thin, since: λ . Vπ = 3 no r63 L The disadvantage of this conﬁguration is the strong birefringence, which induces a very large phase shift in the absence of an applied electric ﬁeld. This birefringence is temperature-sensitive, and the operating point is unstable. To minimize this eﬀect, two identical crystals, rotated by 90◦ around Ox1 , are placed one after the other, so as to cancel the total birefringence. The two crystals must then be submitted to opposite voltages, so that the electrooptical eﬀects add (Exercise 19.1). The two crystals are placed in a thermally insulated box so that they are at the same temperature.

420

Symmetry and Physical Properties of Crystals

19.2.3. Quadratic electro-optical eﬀect, or Kerr eﬀect General properties This eﬀect is much weaker than the linear eﬀect. Therefore, it shows up appreciably only when the linear eﬀect is zero, i.e. in centrosymmetric crystals and in liquids. It is deﬁned by the following relation: ηij (E) − ηij (E = 0) = Δηij = zijkl Ek El where the zijkl are the components of the rank-4 electro-optical tensor, the Kerr tensor [z]. Δηij is symmetric and Ek and El can be interchanged. The matrix of coeﬃcients zijkl can therefore be contracted. The transformation from zijkl to zαβ is performed by writing: ⎛ ⎞ ⎛ ⎞⎛ ⎞ Δη1 z11 z12 z13 z14 z15 z16 E12 ⎜ Δη2 ⎟ ⎜ z21 z22 z23 z24 z25 z26 ⎟ ⎜ E22 ⎟ ⎜ ⎟ ⎜ ⎟⎜ ⎟ ⎜ Δη3 ⎟ ⎜ z31 z32 z33 z34 z35 z36 ⎟ ⎜ E32 ⎟ ⎜ ⎟=⎜ ⎟⎜ ⎟ ⎜ Δη4 ⎟ ⎜ z41 z42 z43 z44 z45 z46 ⎟ ⎜ 2E2 E3 ⎟ . ⎜ ⎟ ⎜ ⎟⎜ ⎟ ⎝ Δη5 ⎠ ⎝ z51 z52 z53 z54 z55 z56 ⎠ ⎝ 2E3 E1 ⎠ Δη6 z61 z62 z63 z64 z65 z66 2E1 E2 Thus zαβ = zijkl whatever α and β, as in the case of the stiﬀness tensor. However, in contrast to the tensors of elasticity, the quadratic electro-optical tensor [z] has no reason to be symmetric with respect to α and β, because no thermodynamic argument can be invoked. Thus, for a triclinic crystal (point groups 1 and ¯1), the 36 coeﬃcients are independent. Tables 19.2a and 19.2b show the various non-zero terms of the tensor as a function of the crystal symmetry. The coeﬃcients of this tensor are expressed in m2 V−2 and are on the order of 10−18 . Application to isotropic materials Most applications of the Kerr electro-optical eﬀect concern isotropic materials such as liquids. To know the form of the tensor, we start out from the tensor for the most symmetrical cubic materials (group m¯3m) and then show, as was done for the stiﬀness coeﬃcients (Sect. 13.6), that the three coeﬃcients z11 , z12 and z44 are connected through relation: 1 z44 = (z11 − z12 ). 2 Suppose we apply an electric ﬁeld E. The form of tensor zαβ is independent of the choice of axes, since the material is isotropic. We can therefore choose the axis directions to suit ourselves, for example take Ox1 parallel to the electric ﬁeld.

Chapter 19 – Electro-optical and elasto-optical eﬀects

421

Table 19.2a: Form of the matrices representing the coeﬃcients zαβ (and pαβ ) for the various point groups P.G.

Triclinic

Monoclinic

1 ¯1

2 m 2 m 2 // Ox2 2 m 2 m 2 // Ox3

Orthorhombic

222 mm2 mmm ⎛

Tetragonal

4 ¯4 4 m

422 4mm ¯42m 4 mm m

⎛ z11 ⎜z21 ⎜ ⎜z31 ⎜ ⎜z41 ⎜ ⎝z51 z61 ⎛ z11 ⎜z21 ⎜ ⎜z31 ⎜ ⎜0 ⎜ ⎝z51 0 ⎛ z11 ⎜z21 ⎜ ⎜z31 ⎜ ⎜0 ⎜ ⎝0 z61 ⎛ z11 ⎜z21 ⎜ ⎜z31 ⎜ ⎜0 ⎜ ⎝0 0

zαβ z12 z22 z32 z42 z52 z62

z13 z23 z33 z43 z53 z63

z14 z24 z34 z44 z54 z64

z12 z22 z32 0 z52 0

z13 0 z23 0 z33 0 0 z44 z53 0 0 z64

z12 z22 z32 0 0 z62

z13 0 z23 0 z33 0 0 z44 0 z54 z63 0

z12 z13 0 z22 z23 0 z32 z33 0 0 0 z44 0 0 0 0 0 0

z11 z12 ⎜z12 z11 ⎜ ⎜z31 z31 ⎜ ⎜ 0 0 ⎜ ⎝ 0 0 z61 −z 61 ⎛ z11 z12 ⎜z12 z11 ⎜ ⎜z31 z31 ⎜ ⎜0 0 ⎜ ⎝0 0 0 0

z15 z25 z35 z45 z55 z65

⎞ z16 z26 ⎟ ⎟ z36 ⎟ ⎟ z46 ⎟ ⎟ z56 ⎠ z66

⎞ z15 0 z25 0 ⎟ ⎟ z35 0 ⎟ ⎟ 0 z46 ⎟ ⎟ z55 0 ⎠ 0 z66 ⎞ 0 z16 0 z26 ⎟ ⎟ 0 z36 ⎟ ⎟ z45 0 ⎟ ⎟ z55 0 ⎠ 0 z66 ⎞ 0 0 0 0⎟ ⎟ 0 0⎟ ⎟ 0 0⎟ ⎟ z55 0 ⎠ 0

z66

⎞ z13 0 0 z16 z13 0 0 −z 16 ⎟ ⎟ z33 0 0 0 ⎟ ⎟ 0 ⎟ 0 z44 z45 ⎟ 0 ⎠ 0 −z 45 z44 0 0 0 z66 ⎞ z13 0 0 0 z13 0 0 0⎟ ⎟ z33 0 0 0⎟ ⎟ 0⎟ 0 z44 0 ⎟ 0 0 z44 0 ⎠ 0 0 0 z66

422

Symmetry and Physical Properties of Crystals Table 19.2b: Form of the matrices representing the coeﬃcients zαβ (and pαβ ) for the various point groups (continued); z ∗ = 12 (z11 − z12 ) P.G.

Rhomboedral

3 ¯3

32 3m ¯3m

Hexagonal

6 ¯6 6 m 622 6mm ¯62m 6 mm m

Cubic

23 m¯3

432 ¯43m m¯3m

Isotropic

⎛

zαβ

⎞ z11 z12 z13 z14 z15 z16 ⎜ z12 z11 z13 −z 14 −z 15 −z 16 ⎟ ⎜ ⎟ z31 z33 0 0 0 ⎟ ⎜ z31 ⎜ ⎟ z44 z45 −z 51 ⎟ ⎜ z41 −z 41 0 ⎝ z −z 51 0 −z 45 z44 z41 ⎠ 51 −z 16 z16 0 −z 15 z14 z∗ ⎛ ⎞ 0 0 z11 z12 z13 z14 0⎟ ⎜z12 z11 z13 −z 14 0 ⎜ ⎟ 0 0 0⎟ ⎜z31 z31 z33 ⎜ ⎟ z44 0 0⎟ ⎜z41 −z41 0 ⎝0 0 0 0 z44 z41 ⎠ 0 0 0 0 z14 z ∗ ⎛ ⎞ 0 0 z16 z11 z12 z13 0 0 −z 16 ⎟ ⎜ z12 z11 z13 ⎜ ⎟ 0 0 0 ⎟ ⎜ z31 z31 z33 ⎜ ⎟ 0 ⎟ 0 0 z44 z45 ⎜ 0 ⎝ 0 0 ⎠ 0 0 −z 45 z44 0 0 z∗ −z 16 z16 0 ⎛ ⎞ 0 0 z11 z12 z13 0 ⎜z12 z11 z13 0 0 0⎟ ⎜ ⎟ 0 0⎟ ⎜z31 z31 z33 0 ⎜ ⎟ 0⎟ 0 0 z44 0 ⎜ 0 ⎝ 0 0 0 0 z44 0 ⎠ 0 0 0 0 0 z∗ ⎛ ⎞ 0 0 z11 z12 z21 0 ⎜z21 z11 z12 0 0 0⎟ ⎜ ⎟ 0 0⎟ ⎜z12 z21 z11 0 ⎜ ⎟ 0⎟ 0 0 z44 0 ⎜0 ⎝0 0 0 0 z44 0 ⎠ 0 0 0 0 0 z44 ⎛ ⎞ 0 0 z11 z12 z12 0 0 0⎟ ⎜z12 z11 z12 0 ⎜ ⎟ 0 0⎟ ⎜z12 z12 z11 0 ⎜ ⎟ 0⎟ 0 0 z44 0 ⎜0 ⎝0 0 0 0 z44 0 ⎠ 0 0 0 0 0 z44 ⎛ ⎞ z11 z12 z12 0 0 0 ⎜z12 z11 z12 0 0 0 ⎟ ⎜ ⎟ ⎜z12 z12 z11 0 0 0 ⎟ ⎜ ⎟ 0 0 z∗ 0 0 ⎟ ⎜0 ⎝0 ∗ 0⎠ 0 0 0 z 0 0 0 0 0 z∗

Chapter 19 – Electro-optical and elasto-optical eﬀects Tensor [Δη] becomes: ⎞ ⎛ ⎛ Δη1 z11 z12 z12 ⎜ Δη2 ⎟ ⎜ z12 z11 z12 ⎟ ⎜ ⎜ ⎜ Δη3 ⎟ ⎜ z12 z12 z11 ⎜ ⎟ ⎜ ⎜ Δη4 ⎟ = ⎜ z44 ⎜ ⎟ ⎜ ⎝ Δη5 ⎠ ⎝ z44 Δη6 z44 and we obtain for tensor [η]: ⎛ 1 2 ⎜ n2 + z11 E ⎜ ⎜ 0 ⎜ ⎝ 0

⎞⎛ ⎟⎜ ⎟⎜ ⎟⎜ ⎟⎜ ⎟⎜ ⎟⎜ ⎠⎝

423

E2 0 0 0 0 0

⎞

⎛

⎟ ⎜ ⎟ ⎜ ⎟ ⎜ ⎟=⎜ ⎟ ⎜ ⎟ ⎜ ⎠ ⎝

z11 E 2 z12 E 2 z12 E 2 0 0 0

⎞ ⎟ ⎟ ⎟ ⎟ ⎟ ⎟ ⎠

⎞ 0

0

1 + z12 E 2 n2 0

0 1 + z12 E 2 n2

⎟ ⎟ ⎟ ⎟ ⎠

where n is the optical index of the liquid. The material is no more isotropic: it has become uniaxial, with the optic axis parallel to the applied electric ﬁeld, and with ordinary index no and extraordinary index ne calculated as in (19.4) since the index change is very small: no = n − n3 z12

E2 2

and

ne = n − n3 z11

E2 . 2

The index ellipsoid is of revolution around the direction of the electric ﬁeld. A Kerr cell contains a liquid to which an electric ﬁeld E is applied normal to the propagation direction of the incident wave (Fig. 19.6a). Two waves propagate in the liquid, one with polarization parallel to E with index ne , the other with index no (Fig. 19.6b). The diﬀerence Δn between the indices is given by: Δn = ne − no = n3 (z12 − z11 ) or

Δn = −n3 z44 E 2 ,

E2 2

(19.11)

which is often written as: ne − no = KλE 2 by setting K=

n3 z44 n3 (z12 − z11 ) =− . 2λ λ

(19.12)

(19.13)

K is the Kerr constant. If the material were not isotropic, but had point group 432 or m¯3 or m¯3m (cubic groups for which the linear electro-optical eﬀect is zero), we would obtain the same result provided the electric ﬁeld is applied parallel to one of the basis vector of the unit cell. The Kerr constant is equal to n3 (z12 − z11 )/2λ (and is no more equal to −n3 z44 /λ).

424

Symmetry and Physical Properties of Crystals x1 + De E

Do

k

x3

x2 –

(a)

(b)

Figure 19.6: (a) Schematic representation of the principle of a Kerr cell; (b) construction of the polarization vectors using the index ellipsoid

19.3. Elasto-optical eﬀects 19.3.1. Deﬁnition Applying stress (tensor [T ]) or a strain (tensor [S]) can lead to a variation [Δη] of the electrical impermeability tensor [η], expressed to ﬁrst order by: Δηij = pijkl Skl , Δηij = πijkl Tkl . The coeﬃcients pijkl and πijkl are those of rank-4 tensors (called elasto-optical tensor and piezo-optical tensor respectively), since each of them connects a rank-2 tensor (the strain tensor [S] or the stress tensor [T ]) to another rank-2 tensor (tensor [Δη]). Tensors [S], [T ] and [Δη] are symmetric. We can therefore contract the coeﬃcients pijkl and πijkl , as was done previously for the elastic tensors and for the Kerr eﬀect tensor. The transformation rules for going from the Sij to the Sα and from the Tij to the Tα make it clear that:

and

pαβ = pijkl παβ = πijkl παβ = 2πijkl

for all α and β for α = 1 to 6 and β = 1 to 3 for α = 1 to 6 and β = 4 to 6.

Matrices pαβ and παβ have no reason to be symmetric with respect to α and β since no thermodynamic argument can be invoked. The eﬀect of crystal symmetry on the number of independent coeﬃcients in tensor [p] is determined in the same way as for the Kerr eﬀect tensor [z]. Table 19.2a and 19.2b are therefore valid for tensor [p] too. The table of independent coeﬃcients for tensor [π] is slightly diﬀerent (Tab. 19.3a and 19.3b) because contraction is not performed the same way.

Chapter 19 – Electro-optical and elasto-optical eﬀects

425

Table 19.3a: Form of the matrices representing coeﬃcients παβ for the various point groups P.G.

Triclinic

1 ¯1

Monoclinic

2 m 2 m 2 // Ox2 2 m 2 m 2 // Ox3

Orthorhombic

Tetragonal

222 mm2 mmm

4 ¯4 4 m

422 4mm ¯42m 4 mm m

⎛

π11 ⎜π21 ⎜ ⎜π31 ⎜ ⎜π41 ⎜ ⎝π51 π61 ⎛ π11 ⎜π21 ⎜ ⎜π31 ⎜ ⎜ 0 ⎜ ⎝π51 0 ⎛ π11 ⎜π21 ⎜ ⎜π31 ⎜ ⎜ 0 ⎜ ⎝ 0 π61 ⎛ π11 ⎜π21 ⎜ ⎜π31 ⎜ ⎜ 0 ⎜ ⎝ 0 0

παβ

⎞ π16 π26 ⎟ ⎟ π36 ⎟ ⎟ π46 ⎟ ⎟ π56 ⎠ π66 ⎞ 0 0 ⎟ ⎟ 0 ⎟ ⎟ π46 ⎟ ⎟ 0 ⎠ π66 ⎞ π16 π26 ⎟ ⎟ π36 ⎟ ⎟ 0 ⎟ ⎟ 0 ⎠

π12 π22 π32 π42 π52 π62

π13 π23 π33 π43 π53 π63

π14 π24 π34 π44 π54 π64

π15 π25 π35 π45 π55 π65

π12 π22 π32 0 π52 0

π13 0 π23 0 π33 0 0 π44 π53 0 0 π64

π15 π25 π35 0 π55 0

π12 π22 π32 0 0 π62

π13 0 0 π23 0 0 π33 0 0 0 π44 π45 0 π54 π55 π63 0 0 π66

⎞ π12 π13 0 0 0 π22 π23 0 0 0 ⎟ ⎟ π32 π33 0 0 0 ⎟ ⎟ 0 ⎟ 0 0 π44 0 ⎟ 0 0 0 π55 0 ⎠ 0 0 0 0 π66

⎛ π11 π12 ⎜π12 π11 ⎜ ⎜π31 π31 ⎜ ⎜ 0 0 ⎜ ⎝ 0 0 π61 −π61 ⎛ π11 π12 ⎜π12 π11 ⎜ ⎜π31 π31 ⎜ ⎜ 0 0 ⎜ ⎝ 0 0 0 0

⎞ π13 0 0 π16 π13 0 0 −π16 ⎟ ⎟ π33 0 0 0 ⎟ ⎟ 0 ⎟ 0 π44 π45 ⎟ 0 ⎠ 0 −π45 π44 0 0 0 π66 ⎞ π13 0 0 0 π13 0 0 0 ⎟ ⎟ π33 0 0 0 ⎟ ⎟ 0 ⎟ 0 π44 0 ⎟ 0 0 π44 0 ⎠ 0 0 0 π66

426

Symmetry and Physical Properties of Crystals Table 19.3b: Form of the matrices representing coeﬃcients παβ for the various point groups (continued); π ∗ = (π11 − π12 ) P.G.

Rhombohedral

3 ¯3

32 3m ¯3m

Hexagonal

6 ¯6 6 m 622 6mm ¯62m 6 mm m

Cubic

23 m¯3

432 ¯43m m¯3m

Isotropic

⎛

παβ

⎞ π15 −2π61 π11 π12 π13 π14 ⎜π12 π11 π13 −π14 −π15 2π61 ⎟ ⎜ ⎟ ⎜π31 π31 π33 0 0 0 ⎟ ⎜ ⎟ ⎜π41 −π41 0 π44 π45 −2π51 ⎟ ⎜ ⎟ ⎝π51 −π51 0 −π45 π44 2π41 ⎠ π61 −π61 0 −π15 π14 π∗ ⎛ ⎞ 0 0 π11 π12 π13 π14 ⎜π12 π11 π13 −π14 0 0 ⎟ ⎜ ⎟ ⎜π31 π31 π33 ⎟ 0 0 0 ⎜ ⎟ ⎜π41 −π41 0 ⎟ π 0 0 44 ⎜ ⎟ ⎝ 0 0 0 0 π44 2π41 ⎠ 0 0 0 0 π14 π ∗ ⎛ ⎞ π11 π12 π13 0 0 −2π61 ⎜π12 π11 π13 0 0 2π61 ⎟ ⎜ ⎟ ⎜π31 π31 π33 0 0 0 ⎟ ⎜ ⎟ ⎜ 0 0 ⎟ 0 0 π44 π45 ⎜ ⎟ ⎝ 0 0 ⎠ 0 0 −π45 π44 0 0 π∗ π61 −π61 0 ⎛ ⎞ 0 0 π11 π12 π13 0 ⎜π12 π11 π13 0 0 0⎟ ⎜ ⎟ ⎜π31 π31 π33 0 0 0⎟ ⎜ ⎟ ⎜ 0 0⎟ 0 0 π44 0 ⎜ ⎟ ⎝ 0 0 0 0 π44 0 ⎠ 0 0 0 0 0 π∗ ⎛ ⎞ 0 0 π11 π12 π13 0 ⎜π13 π11 π12 0 0 0 ⎟ ⎜ ⎟ ⎜π12 π13 π11 0 0 0 ⎟ ⎜ ⎟ ⎜ 0 0 ⎟ 0 0 π44 0 ⎜ ⎟ ⎝ 0 0 0 0 π44 0 ⎠ 0 0 0 0 0 π44 ⎛ ⎞ 0 0 π11 π12 π12 0 ⎜π12 π11 π12 0 0 0 ⎟ ⎜ ⎟ ⎜π12 π12 π11 0 0 0 ⎟ ⎜ ⎟ ⎜ 0 0 ⎟ 0 0 π44 0 ⎜ ⎟ ⎝ 0 0 0 0 π44 0 ⎠ 0 0 0 0 0 π44 ⎛ ⎞ π11 π12 π12 0 0 0 ⎜π12 π11 π12 0 0 0 ⎟ ⎜ ⎟ ⎜π12 π12 π11 0 0 0 ⎟ ⎜ ⎟ ⎜ 0 0 0 π∗ 0 0 ⎟ ⎜ ⎟ ⎝ 0 0 0 0 π∗ 0 ⎠ 0 0 0 0 0 π∗

Chapter 19 – Electro-optical and elasto-optical eﬀects

427

Tensors [p] and [π] are mutually related, since tensors [S] and [T ] are: [S] = [s][T ] and [T ] = [c][S], hence: pijkl = πijmn cmnkl

and

πijkl = pijmn smnkl .

The coeﬃcients pijkl are dimensionless since [S] and [Δη] are, and their maximum value is of the order of 1 (and usually closer to 0.1). The coeﬃcients πijkl are dimensionally reciprocal stresses, and are of the order of 10−12 m2 N−1 . The variation in refractive index, under the eﬀect of stress, is used to analogically evidence stresses in mechanical parts, normally metallic, through the use of models made of transparent and isotropic plastics such as acrylics (Plexiglas , Lucite , Perspex , Altuglas ).

19.3.2. Application to the acousto-optical eﬀects An acoustic wave is a strain wave. In photo-elastic crystals, i.e. those featuring elasto-optical eﬀects, the acoustic wave gives rise to variations in index which it may be of interest to create at will. Consider for example a crystal of lead molybdate, PbMoO4 , with point group 4/m. It is uniaxial, with optical axis parallel to the 4-fold axis. Suppose we excite in this crystal a longitudinal acoustic wave with wave-vector K parallel to the 4-fold axis. This wave creates a displacement u parallel to the 4-fold axis. We choose an orthonormal coordinate system with Ox3 parallel to this 4-fold axis. The longitudinal displacement then has only one component u3 : u3 = a sin(Kx3 − Ωt) where Ω is the angular frequency of the acoustic wave. This displacement induces a strain tensor which has only one non-zero term: S3 =

∂u3 = aK cos(Kx3 − Ωt) = S0 cos(Kx3 − Ωt), ∂x3

where we set, to simplify the expression, S0 = aK. The strain induces a variation in the impermeability tensor given by: ⎞ ⎛ ⎞⎛ ⎞ ⎛ ⎛ p11 0 p12 p13 p16 Δη1 p13 S3 ⎟ ⎜ ⎟ ⎜ Δη2 ⎟ ⎜ p12 ⎜ p p −p p 0 11 13 16 ⎟⎜ ⎟ ⎜ ⎟ ⎜ 13 S3 ⎜ ⎟ ⎜ ⎜ Δη3 ⎟ ⎜ p31 ⎟ ⎜ p p S 31 33 ⎟ ⎜ ⎟⎜ 3 ⎟ = ⎜ p33 S3 ⎜ ⎟ ⎜ ⎜ Δη4 ⎟ = ⎜ ⎟ ⎜ 0 p p 0 44 45 ⎟ ⎜ ⎟⎜ ⎜ ⎟ ⎜ ⎠⎝ 0 ⎠ ⎝ 0 ⎝ Δη5 ⎠ ⎝ −p45 p44 Δη6 p61 −p61 p66 0 0

⎞ ⎟ ⎟ ⎟ ⎟. ⎟ ⎟ ⎠

428

Symmetry and Physical Properties of Crystals

The crystal, when no acoustic wave is excited, has principal indices n1 = n2 = no and n3 = ne , where no and ne are the ordinary and extraordinary indices respectively. With the acoustic wave, tensor [η] becomes: ⎞ ⎛ 1 + p S 0 0 13 3 ⎟ ⎜ n2o ⎟ ⎜ 1 ⎟ ⎜ 0 + p S 0 ⎟. ⎜ 13 3 n2o ⎟ ⎜ ⎠ ⎝ 1 0 0 + p33 S3 . 2 ne The crystal remains uniaxial, with its optic axis parallel to Ox3 , but its ordinary and extraordinary indices have changed to become no and ne respectively. We obtain: 1 1 = 2 + p13 S3 no no2

and

1 1 = 2 + p33 S3 . ne ne2

1 no = no − n3o p13 S0 cos(Kx3 − Ωt), 2 1 3 ne = ne − ne p33 S0 cos(Kx3 − Ωt). 2

Thus

The acoustic wave creates, within the crystal, a modulation of the ordinary and extraordinary indices, periodic along Ox3 , i.e. a grating with period Λ = 2π/K (Fig. 19.7a). The propagation velocity of this index modulation is that of the acoustic wave (V = Ω/K), on the order of a few km s−1 , which is extremely small compared to the propagation velocity of light. During the time it takes light to propagate through the crystal, the grating can therefore be considered as motionless. K

K

E k

x2

O

c

x1

x1 x3

x3

(a)

(b)

Figure 19.7: (a) Schematic representation of diﬀraction of a wave by a crystal of PbMoO4 excited by an acoustic wave with wave-vector K; (b) Bragg diﬀraction on the acoustic grating

Chapter 19 – Electro-optical and elasto-optical eﬀects

429

Suppose we send onto this crystal an optical wave with wave-vector k belonging to plane (Ox1 , Ox3 ), linearly polarized along Ox2 . This wave propagates in the crystal with the index no , modulated by the acoustic wave. It is diﬀracted by this refractive index grating, in the same way as an X-ray wave is diﬀracted by a crystal. The diﬀraction condition for a wave incident on the crystal at an angle θ with the lattice planes can be expressed, as for Bragg “reﬂection” (diﬀraction) (see Sect. 3.2.3), by: 2Λ sin θ = λ/no .

(19.14)

The refractive index does not show up in the expression for X-ray diﬀraction because it is then practically equal to 1. Therefore, the beam is, after diﬀraction, deviated by an angle 2θ when the acoustic wave is excited (Fig. 19.7b). The device is an optical deﬂector. The value of theta is on the order of a degree, as shown by the calculation below. For a crystal of PbMoO4 and an optical wavelength of 500 nm in air, the ordinary index is 2.3. If the acoustic wave has frequency 500 MHz, its propagation velocity in the crystal is 3750 m s−1 . Its wavelength is 7.5 μm. The diﬀraction condition becomes sin θ = 0.0145 and θ = 0.83◦ , so that the deviation of the beam is 1.67◦ . We assumed, as a ﬁrst approximation, that the index grating created by the acoustic wave is ﬁxed. Actually, its motion leads, via the Doppler eﬀect, to a (very small) variation Δω of the diﬀracted wave frequency. This variation is given by: 2V// Δω = ω (c/n) where V// is the projection of the acoustic wave velocity V onto the propagation direction of the optical wave. If the acoustic wave propagates toward the optical wave (as on Fig. 19.7b), Δω is positive, while it is negative in the opposite case. Here V// = V sin θ, and Δω 2V sin θ = . ω (c/n) Taking into account (19.13) and ω = 2πc/λ, Δω =

2πV = Ω. Λ

The diﬀracted wave has an angular frequency ω slightly diﬀerent from ω. ω = ω ± Ω. The + sign corresponds to the case of Figure 19.7, while the − sign corresponds to propagation of the acoustic wave in the opposite direction.

430

Symmetry and Physical Properties of Crystals

This result can be interpreted in terms of particles. An electromagnetic wave with angular frequency ω and wave-vector k is a ﬂow of photons with energy ω and momentum k. The acoustic wave with angular frequency Ω and wavevector K is a set of phonons with energy Ω and momentum K. Diﬀraction of light by the acoustic wave can be viewed as a collision between particles. In the case of Figure 19.7, an incident photon (ω, k) and a phonon (Ω, K) disappear while a new photon (ω , k ) is created. Conservation of energy and of momentum imply: ω = ω + Ω k = k + K. If the acoustic wave were propagating the other way, an incident photon (ω, k) would disappear and a phonon (Ω, K) and a diﬀracted photon (ω , k ) would be created, with ω = ω − Ω k = k − K.

19.4. Exercises Electro-optical eﬀect Exercise 19.1. A block of LiNbO3 (point group 3m) has the shape of a rectangle parallelepiped. Its entrance face is parallel to one of the mirrors and one of the sides of this face is parallel to the 3-fold axis (coinciding with the optic axis). We choose an orthonormal axis set such that Ox3 is parallel to the optic axis and Ox1 is perpendicular to the entrance face. An electric ﬁeld, parallel to Ox3 and pointing toward the positive Ox3 direction, is applied via transparent electrodes deposited on the faces perpendicular to Ox3 (see ﬁgure below).

c O7

x3

x1

E

1.

Show that the crystal remains uniaxial.

2.

A beam of light, perpendicular to the plate and polarized linearly, is sent onto this crystal. Calculate the phase shift ϕ between the components parallel to Ox2 and Ox3 of the electric ﬁeld of the wave, the thickness of crystal traversed being e.

Chapter 19 – Electro-optical and elasto-optical eﬀects 3.

431

After the ﬁrst crystal there is a second crystal, identical to the ﬁrst one (including for the position of the electrodes). It is rotated, with respect to the ﬁrst one, by 90◦ around the propagation direction. It is submitted to an electric ﬁeld with the same norm as that applied to the ﬁrst crystal, but with inverse polarity. Calculate the phase shift ϕ which will add to the phase shift ϕ between the same components of the incident wave. Calculate the thickness e of each crystal so that the total phase shift is equal to π. Numerically: E = 500 V cm−1 ; λ = 633 nm and no = 2.200; ne = 2.286; r13 = 9.6 × 10−12 m V−1 ; r33 = 30.9 × 10−12 m V−1 .

Exercise 19.2 CdTe is a cubic crystal with point group ¯43m. In a system of orthonormal axes parallel to the basis vectors a, b and c, the electro-optical tensor has three nonzero coeﬃcients r41 , r52 and r63 . They are equal: r41 = r52 = r63 = r. For CdTe, r = 4.5 × 10−12 m V−1 . The index n of CdTe for λ = 1 μm is 2.84. An electric ﬁeld E is applied in the [111] direction. 1.

Show that, under this electric ﬁeld, the crystal becomes uniaxial. Determine the direction of the optic axis. Calculate the ordinary and extraordinary indices for E = 2 × 105 V m−1 .

2.

A crystal of CdTe is cut into a rectangle parallelepiped. One of the sides of the entrance face of the crystal is parallel to [111]. An electric ﬁeld is applied parallel to this [111] direction. A beam, with wavelength λ = 1 μm, is perpendicular to the entrance face and traverses this block over a length L = 8 cm. What is the ﬁeld required to obtain a half-wave plate?

Exercise 19.3 ¯ A crystal with point group 42m is optically uniaxial. It is submitted to an electric ﬁeld parallel to the ¯4 axis. Using the Curie principle, determine whether the crystal remains uniaxial. Consider the same question if the crystal has point group 4mm and if the electric ﬁeld is applied parallel to the 4-fold axis. Check the results using the linear electro-optical tensor for each of these point groups.

Elasto-optical eﬀect Exercise 19.4 A crystal of NaCl, with point group m¯3m, is submitted to a uniaxial stress T along direction [1¯10]. 1.

Show that the crystal becomes biaxial. With T = 2 × 108 N m−2 , n0 = 1.54423 and with π11 = 0.25, π12 = 1.46, π44 = −0.85 (in units

432

Symmetry and Physical Properties of Crystals 10−12 m2 N−1 ), calculate the values of the principal indices for this stressed crystal.

2.

The entrance face of the crystal is a (111) surface, and it is illuminated in normal incidence. What are the waves which propagate in the crystal, and what are the corresponding indices?

Exercise 19.5 For point groups 432, ¯43m, m¯3m, show that the variation in refractive index produced by a hydrostatic pressure p is given by: Δn =

n3 (π11 + 2π12 )p. 6

Show that Δn can also be written in the form Δn = (n3 /6) χ (p11 + 2p12 )p, where the pmn are the components of the elasto-optical tensor, and χ the bulk compressibility of the crystal.

Acousto-optical eﬀect Exercise 19.6 Germanium is transparent in the infra-red range, and has point group m¯3m. A transverse acoustic wave, with frequency f = 500 MHz, is excited in a crystal of germanium. The wave, with amplitude A, is polarized along [010] and propagates along direction [001] (see Sect. 14.3.1). Its propagation velocity is given by vt = c44 /ρ and its value is 3580 m s−1 in germanium. 1.

What strain does this wave produce?

2.

Determine the eﬀect on the propagation of a light wave induced by this strain, by calculating (a) the induced index variations, (b) the period of the index grating thus produced.

Chapter 19 – Electro-optical and elasto-optical eﬀects

433

Complement 19C. Frequency doubling, or Second Harmonic Generation (SHG) In this chapter, we investigated the inﬂuence of a static electric ﬁeld on the polarization of a crystal by an electromagnetic wave. This is a special case of a non-linear eﬀect connecting the polarization of a crystal to the electromagnetic ﬁeld(s) that propagate in it. Equation (19.3) can be written, neglecting the spatial dispersion term: Pi (ω) = χij Ej (ω) + χijk Ejs Ek (ω) + . . . ε0 This is a special case of a more general relation: Pi (ω3 ) = χij Ej (ω3 ) + χijk Ej (ω1 )Ek (ω2 ) + . . . ε0 which can be interpreted as follows. If two electromagnetic waves, with angular frequencies respectively ω1 and ω2 , propagate in a crystal, they entail distortions of the electric charge distribution in the crystal, which can oscillate with angular frequency ω3 , a combination of the angular frequencies ω1 and ω2 (ω3 = ω1 ± ω2 ), and thus radiate with the same angular frequency ω3 . The Pockels eﬀect (Sect. 19.2.1) corresponds to ω1 = 0, ω2 = ω and ω3 = ω1 + ω2 = ω. Second harmonic generation corresponds to ω1 = ω2 = ω and ω3 = ω1 + ω2 = 2ω. This phenomenon was evidenced by Franken, Hill, Peters and Weinreich1 in 1961. They focused the beam from a ruby laser (wavelength 694.3 nm) on a quartz crystal, and analyzed the outgoing beam with a prism. They observed, next to the beam with wavelength 694.3 nm, a beam with very low intensity, with wavelength half (347.1 nm) that of the incident beam, hence with twice the angular frequency. The second harmonic yield was then 10−8 . A schematic representation of the experiment is shown on Figure 19C.1. Because χijk is a third-rank tensor property, second harmonic generation is possible only in non-centrosymmetric crystals. Ruby laser

Focusing lens

Quartz crystal

Prism and collimating lenses

694 nm 347 nm

Figure 19C.1: Schematic representation of the setup for second harmonic generation 1. P.A. Franken et al., Generation of optical harmonics, Phys. Rev. Lett. 7 (4), 118 (1961).

434

Symmetry and Physical Properties of Crystals

Using a material more eﬃcient than quartz, a laser with higher intensity, and the phase match property discussed below makes it possible to obtain much better yields. The investigation of the form of the electric ﬁelds shows that the ratio of the powers delivered at the angular frequencies 2ω and ω respectively is proportional to the beam power, to the angular frequency ω, and to the function sin2 ΔkL 2 ΔkL 2

(19C.1)

2

where L is the length of crystal traversed and Δk = k(2ω) − 2k(ω). It is clear that the above function is maximal for Δk = 0 so that k(2ω) − 2k(ω) = 0, which means n(2ω)

ω 2ω = 2n(ω) , c c

so that n(2ω) = n(ω).

(19C.2)

In general, the ordinary and extraordinary indices are increasing functions of ω and relation (19C.2) cannot be satisﬁed if both beams are either ordinary or extraordinary. However, Equation (19C.2) can be satisﬁed by using the ordinary wave at one frequency and the extraordinary wave at the other frequency. For a uniaxial negative crystal (such as KH2 PO4 , also called KDP), no (ω) must have a value between ne (2ω) and no (2ω). There are then directions of the wave-vector for which the ordinary index at angular frequency ω is equal to the extraordinary index at angular frequency 2ω. These directions form a cone of revolution around the optic axis (Exercise 17.6). They are said to produce phase matching. Second harmonic generation (SHG) is widely used, in particular to generate green light at wavelength 532 nm starting with a Nd:YAG laser which emits in the infra-red at 1064 nm.

Further reading G. New, Introduction to Non-Linear Optics (Cambridge University Press, 2011) A. Yariv, Y. Pochi, Optical Waves in Crystals (Wiley, 2003)

Chapter 20

Solutions to the exercises 20.1. Exercises for Chapter 2 Exercise 2.1 The ﬁgure below shows the plane perpendicular to the mirrors going through a given point M. O is the intersection of zz with this plane. M is the transform of M through m1 and M the transform of M through m2 . M”

O

Trace of M2 M’ M

Trace of M1

Figure 20.1 1.

We see that (OM, OM ) = 2α and m2 m1 = Rotzz (2α).

2.

By left-multiplying through m2 , we obtain m1 = m2 Rotzz (2α) since (m2 )2 = E with E being identity. In the same way, by right-multiplying by m1 and using (m1 )2 = E, we obtain m2 = Rotzz (2α)m1 .

3.

The existence of an n-fold axis zz leads to Rotzz (2π/n) being a symmetry operation. m1 is also assumed to be a symmetry operation. So is the product Rotzz (2π/n) m1 = m2 . Therefore there is a mirror M2 enclosing the angle π/n with M1 , etc.

4.

If A is the rotation by π/2 around the axis of the pyramid and m1 , m2 , m3 , m4 the operations of symmetry with respect to each of the 4 mirrors, the 8 symmetry operations are A, A2 , A3 , A4 = E, m1 , m2 , m3 , m4 .

5.

The symmetry group is not commutative. For example m1 m2 = A and m2 m1 = A3 if m1 and m2 are the mirror operations with respect to two mirrors deduced from each other through a 45◦ rotation around zz .

© Springer Science+Business Media Dordrecht 2014 C. Malgrange et al., Symmetry and Physical Properties of Crystals, DOI 10.1007/978-94-017-8993-6_20

435

436

Symmetry and Physical Properties of Crystals

Exercise 2.2 C2 H2 Br2 molecule: a 2-fold axis going through the line that connects the C atoms; 2 orthogonal mirrors going through the 2-fold axis, one containing the H atoms, the other the Br atoms. C3 H4 molecule: the ﬁgure below shows the projection, with the ordinates indicated, of the molecule onto a plane perpendicular to the carbon chain and going through the central C atom. It shows that there is a ¯4 axis going through the line that connects the carbons, with the center of symmetry of the rotoinversions coinciding with the central C atom. There are 2 orthogonal mirrors, with traces M1 and M2 , and two 2-fold axes in the plane of the ﬁgure and at 45◦ to the mirrors. M2 A2(0)

A2(0)

–u

C H

u

u

M1

–u

Figure 20.2

Exercise 2.3 The 4-fold axes are Ox, Oy and Oz, perpendicular to the faces and going through the center O of the cube (Fig. 20.3). The 3-fold axes are the major diagonals of the cube (DF, AG, CE and BH). The 2-fold axes connect the middles of two sides in two opposite faces. Consider, for example, the axis going through M, the middle of BC, and N the middle of EH. MN is parallel to EB. But EB is perpendicular to AF and to AD. Thus it is perpendicular to the plane ADGF. A rotation by π around MN thus transforms the cube apices A, D, G and F into G, F, A and D respectively. It is also clear that this rotation transforms C, B, E and H into B, C, H and E respectively. Thus the cube is transformed into itself. MN is a 2-fold axis.

20.2. Exercises for Chapter 3 Exercise 3.1 1.

The equation of the plane has form hx + ky + lz = n with n an integer. It goes through the nodes (1, 0, 0), (0, 1, 0) and (0, 0, 3), so that h = n, k = n, 3l = n. The required plane is (331).

2.

The (hkl) plane containing [211] and [120] satisﬁes equations 2h+k +l = 0 and h + 2k = 0, so that h = −2k and l = 3k. The plane is (¯213). It contains [302].

Chapter 20 – Solutions to the exercises

437

z D

C M

A

B O y

x

N

H

G

E

F

Figure 20.3 3.

The required row [uvw] satisﬁes equations 3u + v + w = 0 and u − v = 0. Thus u = v and 4u = −w. The row is [11¯4].

Exercise 3.2 1.

The required angle α is the angle between the normals, respectively n1 and n2 , to the planes (101) and (10¯1). n1 = [101]∗ and n2 = [10¯1]∗ . n1 · n2 = n1 n2 cos α with n1 = a∗ + c∗ and n2 = a∗ − c∗ . Since a∗ and c∗ are perpendicular: c2 − a2 a∗2 − c∗2 = = −0.413 and α = 114.4◦ . a∗2 + c∗2 c2 + a2 Another method can be used in this simple case where the planes (101) and (10¯1) are parallel to b and thus perpendicular to the plane of the ﬁgure, (c, a). We see immediately that tan γ = c/a so that γ = 32.8◦ . The angle 2γ = 65.6◦ is the supplement of α. cos α =

_ Trace of (101)

a

c

Trace of (101)

Figure 20.4 2.

In this system a∗ and b∗ are respectively parallel to a and b. Furthermore, a and b have the same norm, and the same applies to a∗ and b∗ . Therefore ha+kb is parallel to ha∗ +kb∗ , hence perpendicular to (hk 0). In contrast, a∗ and c∗ are respectively parallel to a and c but the ratios of their moduli are diﬀerent since a∗ = 1/a and c∗ = 1/c.

438 3.

Symmetry and Physical Properties of Crystals d321 =

1 . Thus d321 = 1.169 Å. 3a∗ + 2b∗ + c∗

Exercise 3.3 1.

(a) The equation of line D is hu + kv = n an integer, u and v being the coordinates of the nodes on D. 2h = n, 3k = n, so that n = 6 and h = 3, k = 2. The equation is 3u + 2v = 6. (b) 5 lines numbered from 1 to 5. (c) The rows have equation 3u + 2v = n. For the row going through node (1, 0), n = 3. For the row going through (0, 1), n = 2 (Fig. 20.5).

N

D

b M O

a

1

2

3

4

5

6

Figure 20.5 2.

(a) The row that goes through M and N is [2¯30]. Plane (hkl) is parallel to c, hence l = 0. It contains [2¯30], hence 2h − 3k = 0. The plane is (320). This result can be retrieved using the above ﬁgure. The lattice plane closest to origin intersects plane (a, b) along the line numbered 1, which intersects a at a/3 and b at b/2. (b) Plane of the form (32). MP parallel to [20¯1], hence = 6, so that the family is (326).

Exercise 3.4 1.

Figure 20.6a below, where c and c∗ are taken to point upwards. √ a∗ = b∗ = 2/a 3; c∗ = 1/c.

2.

Set V∗ = [110]∗ = a∗ + b∗ . (V∗ )2 = (a∗ + b∗ )(a∗ + b∗ ) = a∗2 + b∗2 + 2a∗ · b∗ = 3a∗2

Chapter 20 – Solutions to the exercises

439

Trace of (110) d110

b* b

b * O

a* a

O

(a)

a

(b)

Figure 20.6 since a∗ · b∗ = (a∗ )2 cos γ ∗ = (a∗ )2 /2.

d110

√

2 . a 1 a = = . [110]∗ 2

V∗ =

3a∗ =

This result can, in this special case, be retrieved geometrically using Figure 20.6b. 3.

Let α be the angle between the planes (120) and (100). It is also the angle between the vector [120]∗ , in other words a∗ + 2b∗ , and [100]∗ = a∗ . The calculation is: (a∗ + 2b∗ ) · a* = a∗ + 2b∗ a∗ cos α. √ This yields cos α = 2/ 7 and α = 40.9◦ .

Exercise 3.5 1.

a b

; Area OMN = × h k

a d

area OMQ = × ; h i

d b

area OQN = × . i k

b N

Q M O

a

d

Figure 20.7 2.

Area OMN = area OMQ + area OQN. Since the cross products have the same orientation, we can write: a b a d d b × = × + × h k h i i k

and d = −a − b.

440

Symmetry and Physical Properties of Crystals a×b a×b 1 a×b =− − and =− Therefore: hk hi ik hk hence h + k + i = 0.

3.

1 1 + hi ik

¯ (12¯31) plane; rotation 2π/3 (3121); rotation 4π/3 (2¯311); symmetry with respect to (a, c) (1¯321); symmetry with respect to (b, c) (¯3211).

Exercise 3.6 Unit cell EFGHKLMN. If there were nodes A, B, C and D at the centers of the faces EHNK, EFLK, FGML and HGMN respectively, then AB would be a lattice vector. But AB = NL/2, and there should be a node at the center of face KLMN, so that ﬁnally the lattice would be face-centered. N

M

K A

L D B H

E

C G

F

Figure 20.8 Exercise 3.7 CsCl has a cubic P lattice; the motif is: a pair of neighboring Cs+ and Cl− ions. NaCl has an F-centered cubic lattice; motif: one Na+ and a neighboring Cl− . ZnS has an F-centered cubic lattice; the motif is one Zn2+ and one neighboring S2− . Diamond has an F-centered cubic lattice with the motif: C at (0, 0, 0) and C at (1/4, 1/4, 1/4). CaF2 has an F-centered cubic lattice, with motif: Ca (0, 0, 0) and two F atoms, at (1/4, 1/4, 1/4) and −(1/4, 1/4, 1/4) respectively for example. TiO2 has a tetragonal P lattice, with a motif consisting of two TiO2 groups, one around the Ti at (0, 0, 0) and the other around the Ti at (1/2, 1/2, 1/2). CaTiO3 has a P cubic lattice; the motif is Ca at (0, 0, 0), Ti at (1/2, 1/2, 1/2) and 3 O at the centers of the three faces of the cubic unit cell, viz. at (0, 1/2, 1/2), (1/2, 0, 1/2), (1/2, 1/2, 0). It is clear that an atom in the motif can always be replaced by an identical atom displaced by a lattice vector. For example, in the motif indicated for CaF2 , the F atom at (−1/4, −1/4, −1/4) could be replaced by an F atom at (1/4, −1/4, 1/4) deduced through the lattice mode translation 1/2(a + c), etc. Exercise 3.8 1.

For clarity, the atoms of one layer at height 0 are represented by full circles, connected by full lines forming hexagons. Those of the following layer are represented by empty circles connected by dashed lines which also form hexagons. They are at height 1/2 (Fig. 20.9).

Chapter 20 – Solutions to the exercises

441

d b

height 0 height ½

a

Figure 20.9 2.

The cell is hexagonal, with a value of c equal to twice the distance between layers, viz. c = 6.70 Å. The distance atoms in √ two neighboring √ √ d between a layer is such that d = (2/3)a( 3/2) = a/ 3 and a = 3d = 2.46 Å. There are four atoms per unit cell.

Exercise 3.9 1.

Consider a prism. The two Gd atoms in the bases each is counted for 1/2. The 12 Ni atoms at the apices of the prism each count for 1/6, thus in total 2 atoms. The atoms at the centers of the 6 faces each count for 1/2, thus in total 3. The formula is GdNi5 .

2.

The lattice is hexagonal and the motif, comprising a GdNi5 group, is included in the shaded area on Figure 20.10. #

D

#

#

#

b

#

#

# #

#

C

#

a

B

b

# # #

A #

#

CD

O Gd at height 0 Ni at height 0 # Ni at height ½

a

# #

# #

AB

BC

Figure 20.10 3.

The face parallel to AB is a (110) plane, in hexagonal lattice notation (11¯20). The face parallel to BC is deduced from the face parallel to AB by a rotation through −2π/3 (or 4π/3), and the correct permutation of

442

Symmetry and Physical Properties of Crystals indices (k becomes h, h becomes i) leads to plane (1¯210). In the same way, the face parallel to CD, which is deduced from the face parallel to AB by a rotation through 2π/3, is a (¯2110) plane. These results can be checked on the reduced hexagonal lattice in Figure 20.10: the plane of the family closest to origin, intersecting vector a at a/h and vector b at b/k, has been represented for each face.

4.

The angle between the (1¯10) and (110) planes is equal to 90◦ .

Exercise 3.10 Projection of the nodes of a face-centered tetragonal lattice onto a plane perpendicular to c. 0

½

0

0

½

b ½

0

½

0 a1

b1 0

½

0

½ a

½

0

Figure 20.11 The unit cell deﬁned by the basis vectors a1 , b1 , c, half the size of the F(a,b) unit cell, is centered tetragonal. Note: the same projection applies for an F-centered cubic √ lattice, but then the centered lattice would have a c vector with length 2 times larger than a1 and b1 . It would no more be cubic. Exercise 3.11 Projection of the nodes of a face-centered monoclinic lattice onto a plane perpendicular to c, here chosen parallel to the 2-fold axis. 0

0

½

0

½

b2

½ 0

½

b

½

0

½

0

0

½

0

½

0

½

a1 0

½

b1

a2 0

0

½

½

a

Figure 20.12

0

Chapter 20 – Solutions to the exercises

443

The basis vectors a1 and b1 deﬁne a monoclinic centered unit cell and the vectors a2 and b2 = b1 a base-centered monoclinic unit cell (a2 , c), with B lattice. Exercise 3.12 Line zz , containing the major diagonal K F of the face-centered cubic unit cell, is a 3-fold axis (Fig. 20.13a). A rotation by 2π/3 around this axis changes L into G , G into K and K into L . The middle of L G , R , is transformed into the middle of G K, S , and in the same way S is changed into Q . Line zz therefore intersects the plane P containing the equilateral triangle L G K at its center of gravity I , which is also the center of gravity of the equilateral triangle R S Q . In the same way, zz intersects the plane P containing the equilateral triangle F GL at its center of gravity I. Figure 20.13b is a projection of the planes P and P along zz : the projections of the nodes in plane P are represented by full circles and those of plane P by empty circles. The respective positions of the projections of triangles F GL and L G K, whose centers of gravity I and I project at the same point, are easily deduced from the fact that lines F G and KL , GL and L G , and LF and KG are pairwise parallel. Figure 20.13b is identical to Figure 3.14c if it is complemented by the lattice translations. Since the lattice is face-centered cubic and not rhombohedral, √ the distance between the (111) planes is perfectly deﬁned and equal to a 3/3 if a is the length of the basis vectors. L’

K’

L

z’

R’ F’

L’

G’ I’

S

Q’

S

Q

c

z

S’

I

I

F

R # I’

R’

L b

K

Q'

K R

a

F’

G

S’ Q

G G’

(a)

(b)

Figure 20.13 Exercises 3.13 and 3.14 They should be addressed in the same way as used in the course to determine the reciprocal lattice of a face-centered cubic lattice. For the reciprocal lattice of a body-centered cubic lattice, we obtain a primitive cell with basis vectors A∗ = b∗ + c∗ ,

B∗ = c∗ + a∗ ,

C∗ = a∗ + b∗ ,

444

Symmetry and Physical Properties of Crystals

and thus a face-centered cubic lattice with basis vectors 2a∗ , 2b∗ and 2c∗ . The reciprocal lattice of an A (base-centered) lattice has a primitive cell with basis vectors A∗ = a∗ ,

B∗ = (b∗ − c∗ ),

C∗ = (b∗ + c∗ ).

The lattice is an A-type base-centered lattice, with basis vectors a∗ , 2b∗ and 2c∗ .

20.3. Exercises for Chapter 4 Exercise 4.1 Figure in plane Π : M H M1 V/2

P P’

H’ O V M2

Figure 20.14 O is the middle of M1 M2 = V. MM2 = MM1 + M1 M2 = 2(MH + M1 O) = 2(MH + V/2) = 2MH if HH = M1 O = V/2. Exercise 4.2 Consider a general point M. The ﬁgure is drawn in the plane going through M and perpendicular to zz . The traces of P1 and P2 are represented in this plane. 1.

An elementary geometrical argument shows that M2 is the transform of M through a symmetry with respect to O (Fig. 20.15a). P2 M

O M2

P2

A

M1

M

O

P1 M’1 V

P1 A

M1

M2

(a)

(b)

Figure 20.15 2.

M2 is the transform of M through the product operation (Fig. 20.15b). Line MM2 intersects the trace of P2 at A. Triangles MOA and MM1 M2

Chapter 20 – Solutions to the exercises

445

are similar. Since O is the middle of MM1 , we deduce that A is the middle of MM2 and that OA = M1 M2 /2 = V/2, independently of the choice of point M in the plane. M2 deduces from M through a rotation by π around an axis deduced from zz through a translation by V/2.

20.4. Exercises for Chapter 5 Exercise 5.1 1.

In plane Π, shown on Figure 20.16b, the projection H2 of M2 deduces from the projection H of M by a rotation through 2θ around zz . Also H2 M2 = −H1 M1 = HM, hence M2 deduces from M by a rotation through 2θ around zz . z H2

M2 x’

O

y’

H1

M H

M1

H1

y

x

y

x’

H2

y’

H

x

z’

(a)

(b)

Figure 20.16 2.

A A = R⊥ (2θ). By right-multiplying this equation with A and noting that A2 = E (where E is the identity operation), we ﬁnd: A = R⊥ (2θ)A. In the same way, left-multiplying by A and knowing that A 2 = E, we obtain A = A R⊥ (2θ). If an object has an n-fold axis zz , then Rzz (2π/n) is a symmetry operation for this object. If it additionally has a 2-fold axis perpendicular to zz , the operation of rotation by π around this axis xx , noted A, is also a symmetry operation. So is the product Rzz (2π/n)A. We just showed that Rzz (2π/n) A = A where A is a rotation by π around an axis perpendicular to zz and enclosing with axis xx an angle π/n. Repeating the argument, the object is shown to have n 2-fold axes, perpendicular to zz , and enclosing angles of π/n with each other.

Exercise 5.2 The stereographic projection of a general direction is shown on Figure 20.17a by the cross marked 1. Its transforms through rotations by 2π/3 and 4π/3 around the axis perpendicular to the projection plane are the crosses marked 2 and 3 respectively. The transforms of directions 1, 2 and 3 through the 2-fold axis whose stereographic projection consists of points A and B are the circles

446

Symmetry and Physical Properties of Crystals

marked 4, 5 and 6 respectively. This ﬁgure shows the existence of two 2-fold axes enclosing angles of 2π/3 and 4π/3 with AB (Fig. 20.17b). 6 2

1

A

B 4

5 3

(a)

(b)

Figure 20.17 Exercise 5.3 1.

We choose an orthonormal coordinate system (Oxyz) such that Oy and Oz coincide with the 4-fold axes (the origin O is therefore located at their intersection). We deﬁne the operators for rotation by an angle θ around, say an axis Oy as ROy (θ), which means that, if V is the vector obtained through rotation of a vector V by an angle θ around an axis Oy, then V = ROy (θ) V. The matrices representing the operators for rotations by ±π/2 around Oy or Oz, in the axis system we deﬁned, are given by: ⎛ ⎞ ⎛ ⎞ 0 −1 0 0 1 0 ROz (−π/2) = ⎝ −1 0 0 ⎠ ROz (π/2) = ⎝ 1 0 0 ⎠ 0 0 1 0 0 1 ⎛

⎞ 0 0 1 ROy (π/2) = ⎝ 0 1 0 ⎠ −1 0 0

⎛

⎞ 0 0 −1 ROy (−π/2) = ⎝ 0 1 0 ⎠ . 1 0 0 ⎛ ⎞ 0 0 1 We deduce that ROy (π/2)ROz (π/2) = ⎝ 1 0 0 ⎠. 0 1 0 The composition, or product operation, of a rotation by π/2 around Oz with a rotation by π/2 around Oy is an operation which transforms basis vector i into j, j into k and k into i, i.e. a rotation by 2π/3 around the axis parallel to direction [111] in a cube with sides parallel to Ox, Oy and Oz. The same result can be obtained by considering a cube ABCDEFGH (Fig. 20.18). The rotation by π/2 around Oz transforms: A, B, C, D, E, F, G, H into B, C, D, A, F, G, H, E respectively. The rotation by π/2 around Oy transforms: F, G, C, B, E, H, D, A into G, C, B, F, H, D, A, E respectively.

Chapter 20 – Solutions to the exercises

447

z D

C

A

B

O

y

H E

G F

Figure 20.18 We thus see that, through rotations around Oz, A becomes B and B, through rotation around Oy, becomes F. Thus the composition (product) of the two operations ﬁnally transforms: A, B, C, D, E, F, G, H into F, B, A, E, G, C, D, H respectively. Points B and H remain unaltered, and A becomes F, F becomes C and C becomes A. In the same way, E becomes G, G becomes D, D becomes E. The result is a rotation by 2π/3 around the axis [111] of the cube. In the same way, we can show using either method that: ROy ( π/2 ) ROz ( −π/2 ) = R[1¯11] (−2π/3), ROy ( −π/2 ) ROz ( π/2 ) = R[11¯1] (−2π/3), ROy (−π/2) ROz (−π/2) = R[¯111] (2π/3). Thus the directions [1¯11], [11¯1], [¯111] are also 3-fold axes. We show below the matrices representing rotations by 2π/3 around the four cube diagonals: R[111] (2π/3) ⎞ 0 0 1 ⎝ 1 0 0 ⎠ 0 1 0 ⎛

R[1¯11] (2π/3) ⎛

⎞ 0 −1 0 ⎝ 0 0 −1 ⎠ 1 0 0

R[11¯1] (2π/3) ⎛

⎞ 0 1 0 ⎝ 0 0 −1 ⎠ −1 0 0

R[¯111] (2π/3) ⎛

⎞ 0 −1 0 ⎝ 0 0 1 ⎠ −1 0 0

We recall that the operation inverse to the rotation by 2π/3 around one of these axes is the rotation by −2π/3 around the same axis, and that the associated matrix is the transpose of the matrix of the 2π/3 rotation. 2.

Performing the product of the operation consisting of a ±2π/3 rotation around one of the major diagonals of the cube by the operation consisting

448

Symmetry and Physical Properties of Crystals of a ±2π/3 rotation around another cube diagonal, we obtain a rotation by π around Ox or Oy or Oz. Example: ⎛ ⎞⎛ ⎞ 0 −1 0 0 0 1 R[1¯11] (2π/3)R[111] (2π/3) = ⎝ 0 0 −1 ⎠ ⎝ 1 0 0 ⎠ 1 0 0 0 1 0 ⎛ ⎞ −1 0 0 = ⎝ 0 −1 0 ⎠ 0 0 1 i.e. a rotation by π around Oz.

Exercise 5.4 Let K be the point in the stereographic projection which is located at the intersection of arc bFb and line aa . This point K is the stereographic projection of the direction parallel to row [011] and pointing to the north, i.e. direction OP on Figure 20.19b. This ﬁgure shows the meridian plane containing√direction [011]. We obtain: OK = R tan(π/8) = √ = R tan α = R tan(θ/2) √ R( 2 − 1). Therefore aK = R 2. Since ab = R 2, the circle that goes through b , K and b has for its center a. b’ c’

P

F a

K

a’

a

F’

O

c

K = 45°

b

(a)

(b)

Figure 20.19 Exercise 5.5 Crystals with a hexagonal lattice can have either a hexagonal or a rhombohedral point group. The groups are as follows: Holohedral: 6/mmm, order 24; Hemihedral: ¯62m, 6mm, 622, 6/m and ¯3m with order 12; Tetartohedral: ¯6, 6, 3m, 32, ¯3 with order 6; Ogdohedral: 3, with order 3. The reader can check that the only cases of ogdohedral crystals are those with point group 3 and with a hexagonal lattice. Exercise 5.6 1.

Form {31¯40} (a) Group 6mm: to ﬁnd the faces equivalent to face (hkil) through the symmetry operations of group 6mm, it is suﬃcient to apply the various

Chapter 20 – Solutions to the exercises

449

symmetry elements of the group, viz. rotations by kπ/3 (k being an integer between 1 and 6), and then a mirror operation on the various faces obtained, hence 6 new faces. This gives a total of 12 planes if the normal to the planes is not a special direction. The indices are obtained by remembering that plane hkil intersects axes Ox, Oy and Ov, parallel respectively to a, b and d, at a/h, b/k and d/i. Rotations by 2π/3 and 4π/3 thus produce permutations among h, k and i and conserve l. Rotations by an odd number of ¯ k¯¯il) and the planes deduced through times π/3 lead to the form (h ¯ k¯ and ¯i. permutations among h, (hkil) becomes (ihkl) through a rotation by 2π/3. It becomes (kihl) ¯ through a rotation by through a rotation by 4π/3. It becomes (k¯¯ihl) ¯ kl) ¯ through a rotation ¯ ¯ ¯ π/3, (hk il) through a rotation by π and (¯ih by 5π/3. The operation of a mirror parallel to c and a conserves h and l and exchanges k and i. ¯ (4310), ¯ ¯ ¯ 30), ¯ Form {31¯40} comprises 12 planes: planes (3140), (1430), (14 (3¯¯140), (4¯3¯10) and their transforms through one of the mirrors, (3¯410), (¯4130), (13¯40), (¯1¯340), (¯34¯10), (4¯1¯30). (b) Group ¯62m: the planes equivalent to (31¯40) are obtained by applying ﬁrst the symmetry operations associated to the ¯6 axis, i.e. rotations by 2π/3 and 4π/3 around Oz, and a mirror perpendicular to Oz. The mirror symmetry transforms (hkil) into (hki¯l). Here l = 0 and plane (31¯40) is a special plane because its normal is in the mirror plane. We must also consider the second generating element, which can be either one of the 2-fold axes or one of the mirrors. We choose a mirror, which we take to be parallel to a. Form {31¯40} comprises 6 planes: the planes (31¯40), (¯4310), (1¯430) and (3¯410), (¯4130), (13¯40). 2.

Form {111} for the cubic groups. Form {111} contains the set of faces perpendicular to all the directions equivalent to direction [111]∗ . For a general direction, the number of equivalent directions is equal to the order n of the group. If the direction is located on a symmetry element to which are associated p symmetry operations, the number of equivalent directions is equal to n/p. Direction [111]∗ is a three-fold axis in all the cubic groups. Furthermore, in those groups which also contain diagonal mirrors, i.e. groups ¯43m and m¯3m, it is also located on these mirrors, which divides by another factor 2 the number of equivalent directions. Note that, in this enumeration, it is suﬃcient to consider one of the 3 diagonal mirrors, because the two other mirrors are only the result of the existence of the 3-fold axis and of a mirror going through this axis.

450

Symmetry and Physical Properties of Crystals Group 23: form {111} comprises plane (111) and planes (1¯1¯1), (¯11¯1) and (¯1¯11), obtained by applying the 2-fold axes. It is distinct from form {¯1¯1¯1} because there is no center of symmetry. The latter form contains planes (¯1¯1¯1), (¯111), (1¯11) and (11¯1). We ﬁnd 4 equivalent planes. This number is indeed equal to n/p = 12/3 = 4. Group m¯3: the existence of the mirrors entails the existence of a center of symmetry. The forms {111} and {¯1¯1¯1} are identical and comprise the eight planes (111), (1¯1¯1), (¯11¯1), (¯1¯11) and (¯1¯1¯1), (¯111), (1¯11), (11¯1). We check that this number is equal to n/p = 24/3 = 8. Group 432: although this group does not feature a center of symmetry, the forms {111} and {¯1¯1¯1} are identical because, for this special direction, the product of a rotation by π around Ox and a rotation by π/2 around Oy transforms direction [111]∗ into direction [¯1¯1¯1]∗ . The eight planes are equivalent (n/p = 24/3 = 8). Group ¯43m: same results as for 23. Forms {111} and {¯1¯1¯1} are diﬀerent. The order of the group is 24. Direction [111]∗ is a 3-fold axis and is located on a diagonal mirror, hence 24/6 = 4 equivalent directions. ¯ Group m3m: eight equivalent planes (48/6), and the forms {111} and {¯1¯1¯1} are equivalent because there is a center of symmetry.

20.5. Exercises for Chapter 7 Exercise 7.1 1.

(a) Generating elements: ¯4 and 2-fold axes. The stereographic projection is performed onto a plane perpendicular to the ¯4-axis (Fig. 20.20a). Consider a general direction, with stereographic projection at 1 (cross), and its transforms 2 (circle), 3 (cross), and 4 (circle) through the symmetry operations associated to the ¯4-axis. The 2-fold axis has for its stereographic projection points A and B. The transforms of directions 1, 2, 3 and 4 through rotations by π around the 2-fold axis have stereographic projections 5, 6, 7 and 8 respectively. This shows the existence of the other 2-fold axis and of two mirrors at 45◦ to the 2-fold axes. ¯ Generating elements: 4-axis, and the mirror with the segment MM as its stereographic projection. Same approach: 1, 2, 3 and 4 are the stereographic projections of directions equivalent through the operations associated with the ¯4 axis. 5, 6, 7 and 8 are respectively the stereographic projections of the transforms of directions 1, 2, 3 and 4 through the mirror operation m. This shows the existence of the 2-fold axes located in the projection plane at 45◦ to the projections of the mirrors. The stereographic projection shows very clearly that, if an object has a ¯4 axis and a mirror containing this axis, then there are also 2-fold axes in a plane perpendicular to the ¯4 axis, going through

Chapter 20 – Solutions to the exercises

451

the center of symmetry associated to this ¯4 axis, and enclosing an angle of 45◦ with the traces of the mirrors in this plane (see the C3 H4 molecule of Exercise 2.2). (b) The stereographic projections of the equivalent directions of group 4/mmm, the point group of the tetragonal lattice, are given on Figure 20.20c, where the initial general direction is identical to that in Figures 20.20a and 20.20b. We see that Figures 20.20a and 20.20b represent subgroups of 20.20c. The basis vectors a and b of the lattice are parallel to the mirrors of group 4/mmm, and can therefore be parallel either to the 2-fold axes or to the mirrors of group ¯42m, leading to the space groups P¯42m and P¯4m2 respectively. 2 8 A

7 3

77

2 8 1 5

B

M

7 3

1 5

6 4

6 4

(a)

(b)

P– P42m

7 7

M’

7 7 77

(c)

P– P4m2

Figure 20.20 In order to determine all the symmetry elements present in the unit cell, we apply the rules for the product (composition) of symmetry operations (rotations and rotoinversion) with the lattice translations (Sect. 7.2.3), keeping in mind that a ¯4 axis contains a 2-fold axis. The positions equivalent to the general position with coordinates x, y, z are: ¯ P42m x, y, z y, x ¯, z¯ x ¯, y¯, z y¯, x, z¯ x, y¯, z¯ y, x, z x ¯, y, z¯ y¯, x ¯, z . ¯ P4m2 x, y, z y, x ¯, z¯ x ¯, y¯, z y¯, x, z¯ ¯, z¯ x, y¯, z y, x, z¯. x ¯, y, z y¯, x For both groups, the four positions in the ﬁrst line are obtained by applying the ¯4 operations and their multiples. Those of the second line are obtained by applying to the ﬁrst four positions the operation

452

Symmetry and Physical Properties of Crystals rotation by π around an axis parallel to a for P¯42m, and the operation mirror parallel to a for P¯4m2.

2.

Same approach as in (1). The point group 6/mmm of the hexagonal lattice contains 6 mirrors going through the 6-fold axis, which gives rise to two possibilities for placing the mirrors of point group 3m, a subgroup of the point group of the lattice. If the lattice is rhombohedral, the point group ¯3m of the lattice only has 3 mirrors going through the 3-fold axis. They must coincide with the mirrors in the point group of the crystal.

Exercise 7.2 Group P4 contains a 4-fold axis. We choose the origin of the unit cell on this 4-fold axis, and apply the rules of Section 7.2.3 to obtain the product of the symmetry operations associated to the 4-fold axis with the lattice translations. The rotation by π/2 around the 4-fold axis at A, followed by a translation a, is equivalent to a rotation by π/2 around an axis going through K. There is a 4-fold axis at K. The operation rotation by π around the 4-fold axis going through A followed by a translation a is equivalent to a rotation by π around an axis going through L, the middle of AB = a. There is a 2-fold axis at L, etc. C

K

b

K

b L M

A

L

B

A A

B a I4

a P4

Figure 20.21 Group I4. Existence of a 4-fold axis and a translation 1/2(a + b + c). To perform the product of a rotation by π/2 around the 4-fold axis going through A with the translation, we decompose the translation into its component parallel to the axis, viz. c/2, and its component perpendicular to the axis, 1/2(a + b) = AK. The result is a rotation by π/2 around an axis located at L, the middle of AC = b (the point on the perpendicular bisector of AK at which AK subtends an angle π/2) followed by a translation by c/2. Therefore there exists a 42 axis going through L the middle of AC. The product (composition) of the rotation by π around the 4-fold axis going through A with the translation 1/2(a + b + c) is a rotation by π followed by a translation by c/2 around an axis going through M the middle of AK, hence there exists a 21 axis going through M.

Chapter 20 – Solutions to the exercises

453

Exercise 7.3 The generating elements of this space group are the operations (m1 , c/2) and (m2 , a/2) (modulo the lattice translations). The common origin O of these two operations is located at a point on the intersection of these two mirrors. The product of these two symmetry operations with the same origin is performed by applying relation (4.8). We obtain: (m1 , c/2)(m2 , a/2) = (m1 m2 , m1 a/2 + c/2) = (A, −a/2 + c/2), where A is a rotation by π around the intersection line of the two mirrors. The translation part includes both a component (c/2) parallel to the axis, which is a 21 axis, and a component perpendicular to the axis, (−a/2). The latter can be canceled by displacing the axis: for a 2-fold axis, this implies translating it by −a/4 (ﬁgure below). Thus there is a 21 axis at O such that OO = −a/4. The space group is written Pca21 (c-type mirror perpendicular to a, a-type mirror perpendicular to b, and 21 axis parallel to c). O’ b

O

M1

O’

a

M2

Figure 20.22 Exercise 7.4: Np 1.

Primitive lattice, since the atomic positions cannot be separated into various groups deduced from one another through one (or several) lattice mode translations, such as 1/2(a + b) for a C lattice, etc.

2.

The Np atom at A is located on a 4¯ axis, and we easily see two perpendicular pure mirrors going through A (Fig. 20.23a). The point group of this site is therefore ¯42m. The Np atom at B is on a 4-fold axis and on two orthogonal pure mirrors. The site of atom B has point group 4mm. The point group of the crystal has subgroups ¯ 42m and 4mm. It is therefore 4/mmm.

3.

There is therefore a mirror parallel to the plane of the ﬁgure. It is a glide mirror with translation 1/2(a + b) at height 0 (n-type mirror). The diagonal mirrors going through A are glide mirrors with glide 1/2(a + b) but those which go through B are pure mirrors. The space group is therefore P4/nmm (n◦ 129 in International Tables vol. A). Figure 20.23b shows the

454

Symmetry and Physical Properties of Crystals mirrors present in the unit cell, and the rotation and rotoinversion axes perpendicular to the plane of the ﬁgure. 0

u

u

–u

0

0

u

0

u

–u

0

–u

0

0

–u

A

B

0

B

A

(a)

(b)

Figure 20.23 Exercise 7.5: NiAs Primitive lattice (same reason as in Exercise 7.4, question (1)). A 63 axis going through a Ni atom, 3 pure mirrors going through this 63 axis, and 3 c-type mirrors (glide c/2) intersecting them. Space group P63 mc (n◦ 186 in I.T. A) (the mirrors perpendicular to a and b are m-type mirrors).

1.

½,0

½,0

½,0

u

½,0

u+½

½,0

½,0

u

u

S

u

u+½ ½,0

½,0

b Ni As

½,0

u

½,0

u u+½

½,0

D

R

u+½

a

(a)

b

u+½ ½,0

½,0

u+½ ½,0

b

½,0

u

u u+½

½,0

a

(b)

u+½ ½,0

A

F

K

P

B a

C Q

½,0

(c)

Figure 20.24 Figure (c) shows the symmetry axes and the mirrors present in the unit cell. We apply the rules of Section 7.2.3, taking into account the fact that a 63 axis contains a 3-fold axis and a 21 axis. The combination of the 3-fold axis at P and of the lattice translation a gives a 3-fold axis at point K, while the combination of axis 21 at P and of the lattice translation a gives a 21 axis at B. In order to ﬁnd the eﬀect of the combination of the pure mirror with trace SQ and of the lattice translation a, we decompose a into its component parallel to the mirror, (a − b)/2, and its component perpendicular to the mirror, (a + b)/2. The result is the operation of a

Chapter 20 – Solutions to the exercises

455

mirror with glide (a − b)/2, the trace of which on the plane of the ﬁgure deduces from SQ through a translation by (a + b)/4. We obtain the glide mirror with trace CD (dotted line, see Tab. 7.2). The combination of the c-mirror with trace PR and of the translation with vector a is equivalent to a mirror with trace BC (translation by half the component perpendicular to the mirror of vector a) with glide equal to the component parallel to the mirror of a, viz. (a + b)/2, which adds to c/2 to yield a mirror with trace BC and glide (a +b + c)/2 (dotted line with long/short alternation). The point symmetry of the Ni site is 6mm and that of the As atoms is 3m. Exercise 7.6: FeOCl 1.

Primitive lattice (same reason as in Exercise 7.4, question (1)).

2.

b

w

–u

w

–u

w

u

–w

u

–w

u

w

–u

w

–u

w

Fe

Cl

a w=v

O

w = v’

Figure 20.25 3.

We immediately distinguish two pure mirrors perpendicular to the plane of the ﬁgure and perpendicular to each other. There is a glide mirror with glide vector 1/2 (a + b), parallel to the plane of the ﬁgure at height 0, and therefore a n mirror perpendicular to c. The space group is Pmmn. The associated point group is mmm, a centrosymmetric group. There are therefore symmetry centers. The 2-fold axes parallel to c are pure axes while those parallel to a or b are 21 axes.

4.

There are 8 positions (order of the group = 8) equivalent to the general position. Their coordinates are: x, y, z

x + 1/2, y + 1/2, −z

−x, y, z

−x + 1/2, y + 1/2, −z

x, −y, z

x + 1/2, −y + 1/2, −z

−x, −y, z

−x + 1/2, −y + 1/2, −z.

456

Symmetry and Physical Properties of Crystals

20.6. Exercises for Chapter 8 Exercise 8.1 Figure 3.14b, reproduced below, shows a rhombohedral unit cell. In the closepacked structure ABCABC, points L, N, P and M are the centers of identical, mutually contacting atoms with radius ρ. Then LN = LP = PN = 2ρ. The angle of the rhombohedron is then equal to 60◦ . A rhombohedron with angle 60◦ is the primitive cell for a face-centered cubic lattice. T 3 R S

2

1

Q

N

M

P

0

L

Figure 20.26 Exercise 8.2 1.

Figure 20.27a shows the regular tetrahedron MNPL formed by the centers M, N and P of three mutually contacting atoms in a plane A and the center L of the atom in plane B which contacts them. H, the projection of L onto plane A, is the center of gravity (and orthocenter)√of the equilateral triangle MNP, and MH = (2/3)MK. Also MK = a( 3/2), hence √ MH = a/ 3. L L

h M

O

P a

H

(a)

K N

M

H

(b)

Figure 20.27 In the right triangle LHM, h2 = ML2 – MH2 = a2 (2/3). Hence h = a 2/3.

Chapter 20 – Solutions to the exercises 2.

457

2 = 1.63. c = 2h = 2a 2/3 and c/a = 2 3

Exercise 8.3 1.

2.

3.

We use the ﬁgures and the results of Exercise 8.2. The center O of the tetrahedron with side a is located on the altitude LH, which is a 3-fold axis for the tetrahedron. We must have OL = OM = d (Fig. 20.27b). OH = h − d = a 2/3 − d, OM2 = d2 = MH2 + OH2 = a2 /3 + (a 2/3 − d)2 = d2 . a 3 2 . We deduce from the last equation: a − 2a 2/3d = 0 and d = 2 2 Comparing d and h, we see that d = 3h/4. The center of the regular tetrahedron is located on the height from a vertex, at a distance from the vertex equal to 3/4 of the height. " # a 3 3 d= = r1 + r2 and r2 = a/2 hence r1 = a/2 −1 2 2 2 r1 3 − 1 = 0.225. and = r2 2 The positions of the Zn atoms are those of the centers of an ABABAB stacking. The calculated value of c/a is 1.636. The stacking of the centers is that of close packing, but here the atoms are not in contact. The value of parameter u is close to 0.375 = 3/8. 0

0

0

½ 0

½ 0

0

½ 0

½ 0

0

Figure 20.28 The heights indicated on the ﬁgure are those of the Zn atoms represented by full circles. The S atoms (empty circles) project onto the Zn atoms and are located a distance 3c/8 above them. A Zn atom at height 0 and the 3 neighboring Zn atoms at height 1/2 form a regular tetrahedron with height c/2. The S atom at height 3/8 is a distance 3c/8 from the vertex, hence 3/4 of the height of the tetrahedron. It is therefore at the center of this tetrahedron. The wurtzite structure can thus be represented as an ABABAB stacking, with S atoms in the tetrahedral sites. There is one tetrahedral site per Zn atom. In the blende structure, the Zn atoms form

458

Symmetry and Physical Properties of Crystals an f.c.c. stacking, i.e. an ABCABC stacking. The S atoms are in every other tetrahedral site, since there are twice as many tetrahedral sites as Zn atoms in the f.c.c. structure. We thus understand more clearly why ZnS can exist under these two forms, blende and wurtzite.

20.7. Exercises for Chapter 9 Exercise 9.1 ⎛ 1. 2.

−1 ⎜ √23 {aij }= ⎝ − 2 0

√ 3 2 − 12

0

⎞ 0 ⎟ 0 ⎠ 1

√ T11 = (1/4) T11 + (3/4) T22 − ( 3/2) T12 = T11 √ hence (3/4) (T22 − T11 ) = ( 3/2) T12 , √ = (3/4) T11 + (1/4) T22 + ( 3/2) T12 = T22 T22 √ hence (3/4) (T22 − T11 ) = ( 3/2) T12 , √ = ( 3/4) (T11 − T22 ) − (1/2) T12 = T12 T12 √ hence ( 3/4) (T22 − T11 ) = (−3/2) T12 .

(20.1) (20.2) (20.3)

Relations (20.1) and (20.2) are identical. Relations (20.2) and (20.3) imply that T12 = 0 and T11 = T22 . 3.

√ √ = (−1/2) T13 + ( 3/2)T23 = T13 hence 3 T13 = 3 T23 , T13 √ √ T23 = (− 3/2) T13 − (1/2) T23 = T23 hence 3 T23 = − 3 T13 , = T33 . T33

We deduce that T13 = T23 = 0. Exercise 9.2 Since [T ] is a material tensor, each component must remain unchanged under a symmetry operation of the point group of the crystal, i.e. Tij = Tij . The operation of a mirror perpendicular to Ox1 changes the xi coordinates of a point M into coordinates xj such that: x1 = −x1

x2 = x2

x3 = x3 .

Since the components Tij transform like the product of coordinates xi xj , we obtain: =T , =T , =T , T22 T33 T11 11 22 33 =T . T12 = −T12 = T12 = 0, T13 = −T13 = T13 = 0, T23 23

Chapter 20 – Solutions to the exercises

459

We see that the components Tij with the subscripts ij containing one and only one subscript equal to 1 are zero. The operation of a mirror perpendicular to Ox2 changes the coordinates xi of a point M into coordinates xj such that: x1 = x1

x2 = −x2

x3 = x3 ,

and the components Tij containing one and only one subscript equal to 2 are zero. The existence of a third mirror entails that the components containing one and only one subscript equal to 3 are zero. But these components, T13 and T23 , are already zero because of the ﬁrst two mirrors. We thus note that the form of the tensor is the same for groups mm2 and mmm: ⎞ ⎛ T11 ⎠ ⎝ T22 T33 in an orthonormal set of axes perpendicular to the mirrors.

20.8. Exercises for Chapter 10 Exercise 10.1 ⎛ 1.

2.

⎞ 0 −4 2 0⎠ 0 3 ⎞ 0 4 2 0 ⎠ 0 3

1 {Tij } = ⎝ 0 −4 ⎛ 1 {Tij } = ⎝ 0 4

We could expect to ﬁnd the tensor unchanged, since the basis vector b, perpendicular to a and c, is a 2-fold axis for the three monoclinic groups. Exercise 10.2 ⎛ 1.

⎞ 7 (a) j = ⎝ √0 ⎠ E 3 ⎛ 7+√3 ⎞

⎜ (d) j = ⎝

√

2

0

√ 5+ √ 3 2

⎟ ⎠E

⎛

⎞ 0 (b) j = ⎝ 8 ⎠ E 0 ⎛ √ ⎞ 3

⎛ √ ⎞ 3 (c) j = ⎝ 0 ⎠ E 5 ⎛ √ ⎞ 3

⎜ 2 ⎟ ⎜ 2 ⎟ (e) E = ⎝ 0 ⎠ E ; j = ⎝ 0 ⎠ 8E = 8E, 1 2

1 2

j is parallel to E, and this special direction for E is that of one of the principal axes of the tensor.

460 2.

Symmetry and Physical Properties of Crystals (a) jn = 5E. (b) jn /E = 5 is the value of the electrical conductivity of the material in direction [001].

3.

The coordinate change matrix is given by: √ ⎞ ⎛ 3 1 0 − ⎟ ⎜ 2 2 ⎟ ⎜ ⎜ 0 1 0 ⎟ ⎟. ⎜√ ⎠ ⎝ 3 1 0 2 2 The form of the tensor is therefore: ⎛ 4 8 σ =⎝

⎞ ⎠ 8

and this axis system is that of the principal axes of the tensor. This result is no surprise, since the initial form of the tensor shows that Ox2 is a principal axis. Furthermore, we saw in question 1e) that the direction in plane (Ox3 , Ox1 ) that encloses an angle of 60◦ with Ox3 is a principal axis. Exercise 10.3 ⎛ 1.

{σij } = ⎝

⎞

σ1 ⎛

2.

⎠ (see Sect. 10.5.4).

σ1

σs = (s1 s2 s3 ) ⎝

σ3

⎞⎛

σ1 σ1

⎞ ⎞ ⎛ s1 σ1 s 1 ⎠ ⎝ s2 ⎠=(s1 s2 s3 ) ⎝ σ1 s2 ⎠ σ3 s3 σ3 s 3

= σ1 (s21 + s22 ) + σ3 s23 . s1 = sin θ cos ϕ,

s2 = sin θ sin ϕ,

s3 = cos θ.

σs = σ1 sin2 θ + σ3 cos2 θ. σs is independent of ϕ. This is no surprise since the representative quadric for tensor [σ] has revolution symmetry around the three-fold axis. Exercise 10.4 1.

The symmetry operation associated to the presence of a 4¯ axis parallel to Ox3 is the product of a rotation by π/2 around this axis by a symmetry with respect to origin O. This operation changes the coordinates xi of a point M into coordinates xj such that: x1 = −x2

x2 = x1

x3 = −x3 .

Chapter 20 – Solutions to the exercises

461

The components Tij are expressed as: T11 = T22

T22 = T11

T33 = T33 ,

T13 = T23

T23 = −T13 .

T12 = −T21 = −T12 (symmetric tensor),

Because [T ] is a material tensor, each component must remain unchanged under an operation of the point group of the crystal: Tij = Tij . We deduce: T11 = T22

⎛

The form of tensor [T ] is: ⎝

T12 = 0 T11

T13 = T23 = 0. ⎞ ⎠.

T11 T33

2.

¯ For group 42m, we must add another mirror perpendicular to axis Ox1 . The symmetry operation with respect to the mirror changes the coordinates xi of a point M into coordinates xj such that: x1 = −x1 ,

x2 = x2 ,

x3 = x3 .

This operation leaves the form of the tensor unchanged.

20.9. Exercises for Chapter 11 Exercise 11.1 1.

In a coordinate system (Ox1 x2 x3 ) has the form: ⎛ T ⎝ 0 0

where Ox1 is parallel to n, tensor [T ] ⎞ 0 0 0 0 ⎠. 0 0

In the coordinate system (Ox1 x2 x3 ), the components Tij of the stress = a a T since the only non-zero tensor are given by Tij = aik ajl Tkl i1 j1 = T . The only components which play a role are the term Tij is T11 components ai1 of the matrix for going over from system (Ox1 x2 x3 ) to system (Ox1 x2 x3 ), i.e. the components n1 , n2 , n3 of vector n. We obtain Tij = ni nj T , i.e. the matrix: ⎛ ⎞ n21 n1 n2 n1 n3 ⎝ n1 n2 n22 n2 n3 ⎠ T. n1 n3 n2 n3 n23 Exercise 11.2 1.

Tn = [T ]n. Here only T33 = 0 and (Tn )3 = n3 T and (Tn )2 = (Tn )1 = 0. Tν = Tn · n = n23 T.

462

Symmetry and Physical Properties of Crystals The shear component is the projection of Tn onto the surface. In the plane deﬁned by Tn and n (shown in the ﬁgure): τ 2 = Tn 2 − Tν2 = n23 T 2 − n43 T 2 = n23 T 2 (1 − n23 ), τ = T n3 1 − n23 .

T

Tn n

Figure 20.29 2.

√ 1 − 2n23 ∂τ = T , which vanishes for n3 = ± 2/2. 2 ∂n3 1 − n3 n3 = cos θ where θ is the angle between n and Ox3 . The shear stress is maximal for the orientations of the surface for which the normal is on a cone with axis Ox3 and apical angle 45◦ . Its value is then τ = T /2.

Exercise 11.3 The coordinate change matrix for the axis system is given by: ⎞ ⎛ √ √ 2 2 0 2 2 ⎟ ⎜ √2 √2 ⎝ − 2 0 ⎠. 2 0 0 1 In the new referential, the components Tij form the matrix: ⎛

T ⎝ 0 0

0 −T 0

⎞ 0 0 ⎠. 0

Exercise 11.4 1.

Direction Ox3 is a principal axis, with principal value 7.6. In the subspace (Ox1 , Ox2 ), we solve: det ({Tij } − λE) = 0. We obtain: λ1 = −2, λ2 = 5.5. For λ1 = −2, the principal direction is deﬁned by the relation x1 = −1.33 x2 between its components, so that the direction encloses an angle −36.9◦ with axis Ox1 .

Chapter 20 – Solutions to the exercises

463

For λ2 = 5.5, the principal direction is perpendicular to the above direction. Thus, the principal directions deduce from directions Ox1 and Ox2 through a rotation by −36.9◦ around axis Ox3 . 2.

The position of the center C of the Mohr circle is given by: xC = (2.8 + 0.7)/2 = 1.75 and angle 2θ is deﬁned by: tan 2θ = 3.6/(2.8 − 1.75), so that 2θ = 73.74◦ . Thus the principal directions deduce from directions Ox1 and Ox2 by a rotation through θ = −θ = −36.9◦ around axis Ox3 . P 3.6

2 ’

C –2

O

2.8

5.5

Figure 20.30 3.

√ Let n be the vector ( 3/2, 1/2, 0). We have (Tn )i = Tij nj , so that: ⎞ ⎛ ⎞ ⎛ √3 ⎞ ⎛ ⎞ ⎛ 0.7 3.6 0 2.4 (Tn )1 2 ⎝ (Tn )2 ⎠ = 107 ⎝ 3.6 2.8 0 ⎠ ⎝ 1 ⎠ = 107 ⎝ 4.5 ⎠ 2 0 0 7.6 0 (Tn )3 0 and Tn = 5.1 × 107 N m−2 . The value of the normal stress is: Tν = T · n =

and Tν = 4.3 × 107 N m−2 . The shear stress has value: τ =

√

3 2

1 2

0

⎛

⎞ 2.4 ⎝ 4.5 ⎠ 107 0

Tn 2 − Tν2 = 2.7 × 107 N m−2 .

20.10. Exercises for Chapter 12 Exercise 12.1 ⎛ 1.

⎛ ⎞ ⎞ 2 −1 0 2 12 0 {eij } = ⎝ 2 −2 0 ⎠ 10−5 ; {Sij } = ⎝ 12 −2 0 ⎠ 10−5 ; 0 0 0 0 0 0

464

Symmetry and Physical Properties of Crystals ⎛

0 − 32 {Ωij } = ⎝ 32 0 0 0

⎞ 0 0 ⎠ 10−5 . 0

[Ω] represents a rotation around n (0, 0, 1) through an angle

2.

(see Sect. 12.2.2). ⎛ ⎞ 1 Δ 1 n = √13 ⎝ 1 ⎠ and = ni nj Sij = 10−5 . n 3 1

3 −5 10 rad 2

Exercise 12.2 1.

The displacement vectors Δu = Δr − Δr associated to each side have the following values: ⎛ ⎞ 0 For the side parallel to Ox1 : Δux1 = ⎝ S ⎠. 0 ⎛ ⎞ S For the side parallel to Ox2 : Δux2 = ⎝ 0 ⎠. 0 A square with unit side becomes a lozenge, the major diagonal of which is parallel to the diagonal of the undeformed square (ﬁgure below). x2

S

S O

x1

Figure 20.31 2.

We want to ﬁnd the eigenvalues and eigenvectors of the matrix {Sij } associated to the tensor: ⎛ ⎞ 0 S 0 {Sij } = ⎝ S 0 0 ⎠ . 0 0 0 The eigenvalues are found by solving det ({Sij }−λE) = 0. We obtain three distinct principal values: λ1 = S, λ2 = −S and λ3 = 0. The eigenvector associated to λ1 is parallel to the vector (1, 1, 0), the eigenvector associated

Chapter 20 – Solutions to the exercises

465

to λ2 is parallel to vector (−1, 1, 0). The eigenvector associated to λ3 is along Ox3 . The frame of the principal axes is rotated by 45◦ around Ox3 with respect to the initial frame. In this axis system, the matrix representing the tensor is: ⎛ ⎞ S 0 0 ⎝ 0 −S 0 ⎠ . 0 0 0 Exercise 12.3 ⎛ ⎞ cos α ΔL ⎝ ⎠ = ni nj Sij = η cos2 α − 0.3η sin2 α 1. n = sin α , L n 0 ΔL so that = η(1.3 cos2 α − 0.3). For α < 61.3◦ , L > L. L n ⎛ ⎞ cos α 2. After deformation, Δu = [S]Δr and Δr = ⎝ sin α ⎠ L, so that 0 Δu1 = ηL cos α

and

Δu2 = −0.3ηL sin α.

We project this displacement ⎛ vector Δu ⎞ onto the direction perpendicular − sin α to the direction deﬁned by ⎝ cos α ⎠ (Fig. 20.32). 0 x2 u L

x1

O

Figure 20.32 We obtain: −ηL cos α sin α − 0.3ηL cos α sin α = −1.3η cos α sin αL and the expression for angle ε is: ε = −1.3η cos α sin α = −0.65η sin 2α. Exercise 12.4 ⎛ 4 −1 Sij = ⎝−1 1 2 0

⎞ 2 0⎠ 10−6 , 3

⎛

⎞ 0 3 −4 Ωij = ⎝−3 0 0 ⎠ 10−6 . 4 0 0

466

Symmetry and Physical Properties of Crystals

From the results of Section 12.2.2, the rotation axis is parallel to the unit vector n, with direction cosines n1 , n2 , n3 such that n1 Δα = 0, n2 Δα = −4 × 10−6 and n3 Δα = −3 × 10−6 , where Δα is the rotation angle. The rotation is performed around the direction of unit vector ⎛ ⎞ 0 ⎜ 4⎟ n = ⎝− 5 ⎠ . − 35

We can rewrite matrix {Ωij } in the form: ⎛

0

⎜ 3 ⎝− 5 4 5

3 5

− 45

⎞

0

⎟ 0 ⎠ 5 × 10−6

0

0

and Δα has the value Δα = 5 × 10−6 rad around n. Exercise 12.5 1.

The form of the thermal expansion tensor is ⎞ ⎛ α1 ⎠ ⎝ α1 α3 in an orthonormal set of axes (Ox1 x2 x3 ) where Ox3 is parallel to the basis vector c of the hexagonal structure and Ox1 is any direction in the plane (a, b).

1 a100 − a20 = −1.5 × 10−6 ◦ C−1 , α1 = α2 = a20 ΔT

1 c100 − c20 = 28 × 10−6 ◦ C−1 . α3 = c20 ΔT

2.

Let s be a unit vector with arbitrary direction. Its components in spherical coordinates are: s1 = sin θ cos ϕ,

s2 = sin θ sin ϕ,

s3 = cos θ.

The value of the thermal expansion in direction s is given by: ⎛ ⎞⎛ ⎞ α1 s1 ⎠ ⎝ s2 ⎠ = α1 sin2 θ + α3 cos2 θ. αs = (s1 , s2 , s3 ) ⎝ α1 α3 s3 α3 α3 2 + pπ (p an integer). or θ0 = ± arctan αs = 0 if tan θ0 = − α1 |α1 |

Chapter 20 – Solutions to the exercises

467

By deﬁnition, 0 < θ0 < π and θ0 = 77◦ or θ0 = 103◦ , i.e. all directions on a cone with apex O and apical angle 77◦ . The representative surface for this tensor comprises a one-sheet hyperboloid and a two-sheet hyperboloid. These two hyperboloids are tangent to the same cone with angle 2θ0 and with the apex at the origin of the axes. In the directions of the cone which is the asymptote to the hyperboloids, the relative elongation is zero because the radius vector r tends toward inﬁnity. 3.

We consider the direction ϕ = 0, θ = θ0 i.e. the unit vector s (sin θ0 , 0, cos θ0 ). The displacement vector Δu has components (α1 sin θ0 , 0, α3 cos θ0 ). It is easy to check that Δu · s = α1 sin2 θ0 + α3 cos2 θ0 = 0. The rotation angle ε we want to determine is equal to the norm of Δu. 1/2

cos2 θ0 Δu = (α21 sin2 θ0 + α23 cos2 θ0 )1/2 = |α1 sin θ0 | 1 + tan4 θ0 2 sin θ0 = |α1 sin θ0 | (1 + tan2 θ0 )1/2 = |α1 | |tan θ0 | Thus Δu = 1.3 arcsec ◦ C−1 .

α3 |α1 | and ε is equal to 6.48 × 10−6 rad ◦ C−1

Exercise 12.6 Δa Δc = α11 ΔT and = α33 ΔT . a c Let ϕ be the angle between the planes (100) and (101) (ﬁgure below). ( 10 1) a

O

(100)

c

Figure 20.33 We have: tan ϕ =

a , or ϕ = 57.21◦ . c

Hence: d(tan ϕ) Δϕ 2Δϕ Δa Δc = = = − = (α11 − α33 )ΔT. tan ϕ sin ϕ cos ϕ sin 2ϕ a c We get: α11 − α33 = −2.1 × 10−6 ◦ C−1 . On the other hand, the volume expansion is 23.4 × 10−6 so that: 2α11 + α33 = 23.4 × 10−6 ◦ C−1 .

468

Symmetry and Physical Properties of Crystals

Solving this system of equations, we obtain: α11 = 7.1 × 10−6 ◦ C−1 and α33 = 9.2 × 10−6 ◦ C−1 . Exercise 12.7 1.

Tetragonal phase between 0 and 120◦ C: 1 Δa = 2.3 × 10−5 , ΔT a 1 Δc = = −2.7 × 10−5 . ΔT c

Δa = 0.011 Å and α11 = α22 = Δc = −0.013 Å and α33

The thermal expansion tensor is: ⎛ ⎞ 2.3 ⎝ ⎠ 10−5 ◦ C−1 . 2.3 −2.7 Let n be any direction with direction cosines n1 , n2 and n3 . The value αn of α in direction n is given by: αn = ni αij nj , so that: αn = α11 (n21 + n22 ) + α33 n23 which vanishes for −

α33 n2 + n2 = 1 2 2. α11 n3

If n is expressed in spherical coordinates (θ, ϕ), then tan2 θ = −α33 /α11 = 1.171 and the angle between the direction we want to determine and Ox3 is (±47.3◦ + p 180◦ ), hence 47.3◦ or 132.7◦ . 2.

From Figure 20.34, we have: α bo = bm cos 2 2

co

α co = bm sin . 2 2

bo

cm

bm

Figure 20.34 For the orthorhombic unit cell at T = 0◦ C, α = 90.20◦ and we obtain: ao = 3.988 Å,

bo = 5.664 Å,

co = 5.684 Å.

For the orthorhombic unit cell at T = −100◦ C, α = 90.40◦ and we obtain: ao = 3.978 Å,

bo = 5.654 Å,

co = 5.694 Å.

Chapter 20 – Solutions to the exercises

469

The thermal expansion tensor in the orthorhombic phase can be written, in the orthonormal axis system parallel to the basis vectors of the orthorhombic unit cell: ⎛ ⎞ 2.5 ⎝ ⎠ 10−5 ◦ C−1 . 1.8 −1.8 3.

(a) Cubic ↔ tetragonal transition at 120◦ C: In an orthonormal axis system parallel to the basis vectors of the cubic unit cell, the strain tensor is: ⎛ ⎞ −2 ⎝ ⎠ 10−3 . −2 2.7 (b) Strain tensor describing the transition from the cubic unit cell at 120◦ C to the orthorhombic unit cell at 0◦ C: The orthorhombic unit cell must be compared with the equivalent unit cell in the cubic phase, i.e. with a double unit cell with basis vectors a , b and c . a is parallel to a and a = 4.010 Å, b and c are parallel respectively to the diagonals of the (b, c) faces, and such that √ b = c = a 2 = 5.671 Å. The strain tensor is diagonal in an axis system parallel to the basis vectors of the orthorhombic unit cell, and: ao − a = −5.5 × 10−3 , a co − c = = 2.2 × 10−3 . c

S11 = S33

S22 =

bo − b = −1.2 × 10−3 , b

The strain tensor, when expressed in the axis system of the orthorhombic unit cell, is thus ⎛ ⎞ −5.5 ⎝ ⎠ 10−3 . −1.2 2.2 (c) Strain tensor describing the transition from the cubic unit cell to the rhombohedral unit cell: When going over from the cubic unit cell to the rhombohedral unit cell, the [111] axis of the cube remains a 3-fold axis, and the mirrors containing this axis (the diagonal mirrors of the cube) remain mirrors for the rhombohedral unit cell. The basis vectors a = OA and c = OC of the cubic unit cell become vectors OA and OC such that: ⎧ ⎧ √ ϕ2 2 ⎪ ⎪ ⎨ a (1 −√ 2 ) ⎨ a ϕ √2 and OC OA a ϕ √22 a ϕ 22 ⎪ ⎪ 2 ⎩ ⎩ 2 aϕ 2 a (1 − ϕ2 )

470

Symmetry and Physical Properties of Crystals where ϕ is the angle of rotation of a, b and c in their respective diagonal mirror (Fig. 20.35).

C

c

C’

B’ B

b a

O

A’ A

Figure 20.35

S11 = S22 = S33 = √ 2 . S12 = S13 = ϕ 2

a − a a (1 − ϕ2 /2) − a ≈ = −3.5 × 10−3 . a a

Calculating angle of α, we obtain OA · OC = √ ϕ as a function cos α 2 2 √ a cos α = a ϕ 2 and ϕ = 2 . cos α = 1.2 × 10−3 . 2 The component S23 is obtained in the same way.

Thus S12 = S13 =

The strain tensor describing the transition from the cubic unit cell to the orthorhombic unit cell, expressed in the axis system parallel to the basis vectors of the cubic unit cell, is: ⎛ ⎞ −3.5 1.2 1.2 ⎝ 1.2 −3.5 1.2 ⎠ 10−3 . 1.2 1.2 −3.5

20.11. Exercises for Chapter 13 Exercise 13.1 By adding to the symmetry elements of group ¯42m a 3-fold axis parallel to the major diagonal of a cube with sides parallel to the basis vectors a, b and c, we obtain point group ¯43m. Such a symmetry operation changes the coordinates xi of a point M into coordinates xj such that: x1 = x2 We obtain: s11 = s22 = s33 ,

x2 = x3

x3 = x1 .

s44 = s55 = s66 ,

s12 = s13 = s23 .

Chapter 20 – Solutions to the exercises

471

Exercise 13.2 1.

We choose an orthonormal axis system (Ox1 x2 x3 ) parallel to the basis vectors a, b and c of the cubic unit cell. From the generalized Hooke’s law, Sα = sαβ Tβ with T1 = T and T2 = T3 = T4 = T5 = T6 = 0. The resulting strain tensor is: ⎞ ⎛ s11 ⎠ T. ⎝ s12 s12 The relative elongation in direction [100] is s11 T .

2.

In the axis system (Ox1 x2 x3 ), rotated through 45◦ around Ox3 with re = T and that spect to the initial frame, the stress tensor is such that T11 the other components are zero. In the frame (Ox1 x2 x3 ) linked to ⎛ T /2 ⎝ T /2 0

the cube axes, this tensor becomes: ⎞ T /2 0 T /2 0 ⎠ 0 0

and the strain tensor is thus:1 ⎛ s44 s11 + s12 2 ⎜ s44 Sij = ⎜ + s12 s 11 ⎝ 2

⎞ ⎟T ⎟ . ⎠2 2s12

The relative elongation in direction [110] is obtained through relation (12.12): Δ = wi wj Sij . w T Δ = [2(s11 + s12 ) + s44 ]. We obtain: [110] 4 3.

If the solid is isotropic, these two strains must be identical, so that: 1 [2(s11 + s12 ) + s44 ] = s11 4

or

s44 = 2(s11 − s12 ).

Exercise 13.3 We directly apply the generalized Hooke’s law (relation (13.1a)): Sα = sαβ Tβ with T1 = T2 = T3 = −p and T4 = T5 = T6 = 0, using the elasticity tensor for group 4/mmm given in Table 13.5. We obtain : ⎞ ⎛ s11 + s12 + s13 ⎠. s11 + s12 + s13 −p ⎝ 2s13 + s33 1. We recall that S12 = S21 = S6 /2.

472

Symmetry and Physical Properties of Crystals

The numerical values are: S11 = S22 = −0.61 × 10−4 ; S33 = −0.68 × 10−4 ΔV and = S11 + S22 + S33 = −1.9 × 10−4 . V Exercise 13.4 We consider a uniaxial stress T , parallel to a direction w with direction cosines w1 , w2 and w3 . In an orthonormal axis system (Ox1 x2 x3 ) where Ox1 is = T. parallel to w, the stress tensor has a single non-zero component, T11 Let Tij be the components of this tensor in the axis system (Ox1 x2 x3 ) parallel to the cube axes. We have Tmn = aim ajn Tij where {aij } is the transformation matrix for going over from system (Ox1 x2 x3 ) to system (Ox1 x2 x3 ). =a Here Tmn = a1m a1n T11 1m a1n T with a11 = w1 , a12 = w2 and a13 = w3 .

T11 = w12 T,

T22 = w22 T,

T33 = w32 T,

T12 = w1 w2 T, T13 = w1 w3 T, T23 = w2 w3 T. We showed (Sect. 12.4) that:

ΔV = S11 + S22 + S33 . V

S11 = s11 T11 + s12 (T22 + T33 ) = s11 w12 T + s12 T (w22 + w32 ),

S22 = s11 T22 + s12 (T11 + T33 ) = s11 w22 T + s12 T (w12 + w32 ), S33 = s11 T33 + s12 (T11 + T22 ) = s11 w32 T + s12 T (w12 + w22 )

ΔV = [s11 (w12 + w22 + w32 ) + 2s12 (w12 + w22 + w32 )]T = (s11 + 2s12 ) T V since w12 + w22 + w32 = 1.

and

Exercise 13.5 It was shown in Section 13.7 that, in the cubic system, the reciprocal of Young’s modulus in a given direction, deﬁned by unit vector w with components w1 , w2 and w3 , is given by: 1 s44 2 2 (w2 w3 + w12 w22 + w12 w32 ) = A. = s11 − 2 s11 − s12 − Ew 2 Ew has its maximum value if A is minimum. If s11 − s12 − s44 /2 is positive, A is minimum if B = w22 w32 + w12 w22 + w12 w32 is maximum. In spherical coordinates (θ, ϕ), the components of w are: w1 = sin θ cos ϕ, 2

w2 = sin θ sin ϕ, 4

w3 = cos θ

sin θ sin 2 θ + sin2 2 ϕ . 4 4 B is the sum of two terms which are always positive, and only the second term depends on ϕ. Therefore B is maximum, whatever the value of θ is, when sin2 2ϕ is maximum, hence for 2ϕ = π2 + pπ i.e. ϕ = π4 + p π2 .

and

B=

Chapter 20 – Solutions to the exercises For this value of ϕ,

B=

473

sin2 2 θ sin4 θ + . 4 4

dB = cos 2θ sin 2θ + cos θ sin3 θ dθ = 2 cos3 θ sin θ − sin3 θ cos θ = sin θ cos θ(3 cos2 θ − 1).

√ = 0 for θ = 0, θ = π/2 and for θ such that cos θ = 1/ 3, thus θ = 54.7◦ , which is the angle between direction [111] and Ox3 in the cubic system. dB dθ

For θ = 0 : π For θ = : 2 Pour θ = 54,7◦ :

B=0 B = 1/4 B = 1/3, the maximum value.

This shows that the value of Young’s modulus for a cubic material is extremal in direction [111]. Exercise 13.6 In an orthonormal coordinate system (Ox1 x2 x3 ) where direction Ox1 is parallel to the [110] direction of the cubic lattice, the stress tensor has only one non-zero = T. component, T11 In the orthonormal frame (Ox1 x2 x3 ) with the cubic unit cell, this tensor becomes: ⎛ T /2 T /2 ⎝ T /2 T /2 0 0

axes parallel to the basis vectors of ⎞ 0 0 ⎠. 0

The resulting strain is given, in the axis system of the cube, by: ⎛ ⎞ s44 s11 + s12 2 ⎜ ⎟T s44 ⎟ . Sij = ⎜ s11 + s12 ⎝ ⎠2 2 2s12 We recall that S6 = 2S12 = 2S21 . The relative elongation in a given direction is given by (12.12): Δ = wi wj Sij . w Δ = w12 S11 + w22 S22 + 2w1 w2 S12 + w32 S33 . We obtain: Here, w Δ Δ T s44 s11 + s12 + , = = s12 T, [110] 2 2 [001] T s44 Δ s . = + s − 11 12 [1¯10] 2 2

474

Symmetry and Physical Properties of Crystals

Numerically: s12 = −6× 10−13 m2 N−1 , s11 = 9.6× 10−12 m2 N−1 , s44 = 78× 10−12 m2 N−1 . Exercise 13.7 1.

The uniaxial stress applied to the crystal is parallel to direction [111], with √ unit vector w, with direction cosines w1 = w2 = w3 = 1/ 3. In a coordinate system where Ox1 is parallel to [111], the only non-zero = T . In the orthonormal coordinate component of the stress tensor is T11 system with axes parallel to the basis vectors of the cubic unit cell, this tensor becomes (see the solution to Exercise 11.1): ⎞ ⎛ T T T 1⎝ T T T ⎠. 3 T T T

2.

The resulting strains are: S1 = S2 = S3 =

3.

T (s11 + 2s12 ), 3

S4 = S5 = S6 =

T s44 . 3

The basis vectors a, b, c of the cubic unit cell become respectively, after deformation, the vectors a , b , c such that ⎛ ⎛ ⎛ ⎞ ⎞ ⎞ 1 + S1 S6 /2 S6 /2 a = ⎝ S6 /2 ⎠ a, b = ⎝ 1 + S1 ⎠ a, c = ⎝ S6 /2 ⎠ a. S6 /2 S6 /2 1 + S1 We note that the components of these vectors can be deduced from one another by circular permutation. Therefore these vectors deduce from one another by rotation through 2π/3 around direction [111]. The unit cell has become rhombohedral. The parameter a of the rhombohedral unit cell is given by: T a = a(1 + S1 ) = a 1 + (s11 + 2s12 ) . 3 a · b = a b cos γ . Neglecting the second order terms, we obtain: cos γ = S6 = cos(π/2 − ε) = sin ε,

so that

ε = S6 =

T s44 . 3

Exercise 13.8 1.

In an orthonormal coordinate system (Ox1 x2 x3 ) with axes parallel to the sides of the parallelepiped, the uniaxial stress has only one non-zero component, T11 = −T . The resulting strain tensor is: ⎞ ⎛ s11 ⎠ T. s12 −⎝ s12

Chapter 20 – Solutions to the exercises

475

ΔL = −s11 T = −1.49 × 10−2 and ΔL = −74.5 μm L Δ = −s12 T = 0.63 × 10−2 and Δ = 6.3 μm. The orthonormal axis system (Ox1 x2 x3 ), with axes parallel to the sides of the rectangle parallelepiped, is deduced from the crystallographic axis system (Ox1 x2 x3 ) by a rotation through +45◦ around Ox3 . In the axis system (Ox1 x2 x3 ), the tensor has only one non-zero component, T11 = −T . In the coordinate system (Ox1 x2 x3 ), this tensor becomes ⎛ ⎞ −T /2 −T /2 ⎝ −T /2 −T /2 ⎠. 0 As a result,

2.

The components of the corresponding strain tensor are:

T = S2 , S3 = −s12 T, S1 = (s11 + s12 ) − 2 T and S6 = − s44 . S4 = S5 = 0 2 In the coordinate system (Ox1 x2 x3 ), these components become: T S1 = − [2(s11 + s12 ) + s44 ] = −0.76 × 10−2 , 4 T S2 = − [2(s11 + s12 ) − s44 ] = 0.63 × 10−2 , 4 S3 = −s12 T = 0.975 × 10−3 . S4 = S5 = S6 = 0. Since the non-diagonal terms are zero, the rectangle parallelepiped remains a rectangle parallelepiped. The sides AB and BC have changed respectively by Δ(AB)= −7.6 μm and Δ(BC) = 6.3 μm. Length L has changed by ΔL = 0.49 μm.

20.12. Exercises for Chapter 14 In all exercises, use is made of Table 14.1 to determine the Christoﬀel matrix, and of Tables 13.5a and 13.5b to know which components of the stiﬀness tensor [c] are non-zero. Exercise 14.1 1.

(a) k is parallel to [001]. In the orthonormal coordinate system (Ox1 x2 x3 ) where Ox3 is parallel to c, s1 = s2 = 0 and s3 = 1, so that Christoﬀel’s matrix is given by ⎞ ⎛ c55 c45 c35 ⎝ c45 c44 c34 ⎠ . c35 c34 c33

476

Symmetry and Physical Properties of Crystals From Table 13.5a, c35 = c34 = 0 ⎛ c55 ⎝ c45 0

and the matrix becomes: ⎞ c45 0 c44 0 ⎠ . 0 c33

(b) The propagation velocities are obtained from the eigenvalues of this matrix. They are given by: λ1 λ2 and v2 = v1 = ρ ρ with λ1,2 =

c44 + c55 ±

(c44 − c55 )2 + 4c245 , 2 c33 . v3 = ρ

The wave which propagates at velocity v3 is polarized parallel to direction [001]: it is a longitudinal wave. The waves which propagate with velocities v1 and v2 are transverse waves. The polarization of the wave with velocity v1 encloses with direction Ox1 , in plane (Ox1 ,Ox2 ), an angle θ1 such that:

(c44 − c55 ) − (c44 − c55 )2 + 4c245 λ1 − c55 θ1 = arctan = arctan . c45 2c45 The polarization of the wave with velocity v2 encloses with direction Ox1 the angle θ2 such that:

λ2 − c55 . θ2 = arctan c45 We check that θ2 − θ1 = π/2. 2.

For the orthorhombic system, c45 = 0 (see Tab. 13.5a). Christoﬀel’s matrix takes the form: ⎞ ⎛ c55 0 0 ⎝ 0 c44 0 ⎠ . 0 0 c33 Waves with polarization parallel to Ox1 and Ox2 , hence transverse, propagate with the respective velocities v1 and v2 , given by: c55 c44 v1 = and v2 = . ρ ρ

Chapter 20 – Solutions to the exercises

477

The wave with polarization parallel to Ox3 , hence longitudinal, propagates with velocity v3 given by: c33 v3 = . ρ 3.

Christoﬀel’s matrix is : ⎞ c55 c45 c35 ⎝ c45 c44 c34 ⎠ . c35 c34 c33 ⎛

From Tables 13.5a and 13.5b, all point groups with an axis of order larger than 2 feature c45 = c35 = c34 = 0. Furthermore, c44 = c55 . Christoﬀel’s matrix thus becomes: ⎛ ⎞ c44 ⎝ ⎠. c44 c33 There is a longitudinal wave, with propagation velocity v given by: c33 v = . ρ The transverse waves have their polarization along any direction in the plane (Ox1 , Ox2 ) and they propagate with velocity vt given by: c44 vt = . ρ 4.

For a general propagation direction in plane (Ox1 , Ox2 ), we have: s1 = 0, s2 = 0 and s3 = 0. Christoﬀel’s matrix is: ⎞ ⎛ Γ11 Γ12 ⎠ ⎝ Γ12 Γ22 Γ33 since Γ13 = Γ23 = 0 for a hexagonal crystal. Here: Γ11 = c11 s21 + c66 s22 ,

Γ22 = c66 s21 + c22 s22 ,

Γ33 = c55 s21 + c44 s22 = c44 (s21 + s22 ) = c44 , Γ12 = (c12 + c66 )s1 s2 . One wave with polarization parallel to the 6-fold axis can propagate. It is transverse, with propagation velocity given by: c44 . v= ρ

478

Symmetry and Physical Properties of Crystals

Exercise 14.2 1.

k is parallel to [100], hence s1 = 1, s2 = s3 = 0, and Christoﬀel’s matrix contains only 3 coeﬃcients: Γ11 = c11 , Γ22 = c44 , Γ33 = c44 . One longitudinal wave can propagate, with velocity v given by: c11 v = . ρ The transverse waves have any polarization direction in the plane (Ox2 , Ox3 ), and their propagation velocity vt is given by: c44 . vt = ρ

2.

√ k is parallel to [111], hence s1 = s2 = s3 = 1/ 3, and Christoﬀel’s matrix takes the form: ⎞ ⎛ c + 2c44 c12 + c44 c12 + c44 1 ⎝ 11 c12 + c44 c11 + 2c44 c12 + c44 ⎠ . 3 c12 + c44 c12 + c44 c11 + 2c44 The propagation velocities are obtained from det({Γij } − λE) = 0. If we set (c11 + 2c44 )/3 = a and (c12 + c44 )/3 = b: det({Γij } − λE) = (a − λ)[(a − λ)2 − b2 ] − b2 [a − λ − b] + b2 [b − (a − λ)]. We must solve: (a − λ)(a − λ + b)(a − λ − b) − 2b2 (a − λ − b) = 0, (a − λ − b)[(a − λ)(a − λ + b) − 2b2 ] = 0. We ﬁnd λ1 = a − b and λ2 − λ(2a + b) + a2 + ab − 2b2 = 0, so that λ2 = a − b = λ1 and λ3 = a + 2b. The eigenvector associated to λ3 = a + 2b turns out to be parallel to [111], so that the wave is longitudinal with propagation velocity: c11 + 2c12 + 4c44 v = . 3ρ The other two eigenvalues are equal and correspond to transverse waves with any polarization direction in the plane perpendicular to [111]. Their propagation velocity is given by: c11 − c12 + c44 . vt = 3ρ

Chapter 20 – Solutions to the exercises 3.

479

Numerically: The velocity of the transverse waves found in question (1) yields c44 : c44 = 4.40 × 1011 N m−2 . c11 and c12 are determined from the results of (2): c11 + 2c12 = 3ρv2 − 4c44 c11 − c12 = 3ρvt2 − c44 . We ﬁnd: c11 = 10.9 × 1011 N m−2 and c12 = −3.18 × 1011 N m−2 .

Exercise 14.3 1 The wave-vector k is parallel to [110]: s1 = s2 = √ and s3 = 0. 2 ⎞ ⎛ 0 c + c66 c12 + c66 1 ⎝ 11 Christoﬀel’s matrix is: 0 ⎠. c12 + c66 c11 + c66 2 0 0 2c44

c11 − c12 c11 + c12 + 2c66 −λ −λ . det({Γij } − λE) = (c44 − λ) 2 2 The propagation velocities are obtained from det({Γij } − λE) = 0. Here c44 is an eigenvalue with eigenvector [001]. c44 , polarization [001], transverse wave; We ﬁnd: v1 = ρ c11 − c12 v2 = , polarization [¯110], transverse wave; 2ρ c11 + c12 + 2c66 v3 = , polarization [110], longitudinal wave. 2ρ

20.13. Exercises for Chapter 15 Note: in this section, the coeﬃcients of the piezoelectric tensors which vanish are represented by small dots. Exercise 15.1 The piezoelectric tensor for group 422 has the following form in an orthonormal axes system (Ox1 x2 x3 ) where Ox3 is parallel to the 4-fold axis and Ox1 and Ox2 are parallel to the 2-fold axes: ⎛ ⎞ . . . . . d14 ⎝. . . . − d14 . ⎠ . . . . . . 0 To determine the form of the tensor for group 432, we just have to add a 3-fold axis, parallel to the diagonal of the cube, because the 2-fold axes perpendicular

480

Symmetry and Physical Properties of Crystals

to the diagonal planes result from the existence of the 4-fold and 3-fold axes. We then use the direct inspection method applied to a rotation by 2π/3 around the major diagonal of the cube. This operation changes the coordinates xi of a point M into coordinates xj such that: x1 = x2 ,

x2 = x3 ,

x3 = x1 .

We obtain: d14 = 2d132 = 2d213 = d25 = −d14 = d14 ,

whence d14 = 0.

Exercise 15.2 1.

(a) We consider the stereographic projection of the equivalent directions for group 222 (Fig. 20.36a). The Ox1 axis is parallel to one of the 2-fold axes. If we add the operation of symmetry with respect to a mirror enclosing an angle of 45◦ with Ox1 , we add the equivalent directions 5, 6, 7 and 8, which are the transforms of directions 1, 2, 3 and 4 respectively. We see that this leads to group ¯42m. 6 5 3 4

1 2

x1

3 4

1 2 8 7

(a)

(b)

(c)

Figure 20.36 The form of the piezoelectric tensor for group 222 (in an orthonormal set of axes parallel to the 2-fold axes) is (Tab. 15.2): ⎞ ⎛ . . . . d14 . ⎝. . . . d25 . ⎠ . . . . . . d36 The operation of symmetry with respect to the mirror changes the coordinates xi of a point M into coordinates xj such that: x1 = x2 ,

x2 = x1 ,

x3 = x3 .

This leads to d132 = d231 = d132 whence d25 = d14 . The transformation of d312 tensor is: ⎛ . . ⎝. . . .

yields nothing more. The form of the ⎞ . . d14 . . . d14 . ⎠ . . . . d36

Chapter 20 – Solutions to the exercises

481

(b) In the same way, considering subgroup mm2, the addition of the rotation by π around an axis at 45◦ to the mirrors leads to group ¯42m. The form of the tensor for group mm2 (in an orthonormal system with axes perpendicular to the mirrors) is: ⎞ ⎛ . . . . d15 . ⎝ . . . d24 . .⎠ . . . d31 d32 d33 . A rotation by π around an axis at 45◦ to the mirrors changes coordinates xi of a point M into coordinates xj such that: x1 = x2 ,

x2 = x1 ,

x3 = −x3 .

Therefore: d131 = −d232 = d131 whence d15 = −d24 ;

d311 = −d322 = d311 whence d31 = −d32 ; d333 = −d333 = d333 whence d33 = 0. The form of the tensor is: ⎛ ⎞ . . . . d15 . ⎝ . . . −d15 . .⎠ . . . . d31 −d31 . 2.

The tensor which we obtained in (1a), relative to an axis system (Ox1 x2 x3 ), must now be expressed in a new axis system (Ox1 x2 x3 ), deduced from the ﬁrst one through a rotation by 45◦ around axis Ox3 . Knowing the form of the tensor in the new axes reduces the task to the calculation of two of them: d15 and d31 . We apply the rule dijk = ail ajm akn dlmn , √ ⎛ √ 2 2 ⎜ 2 2 ⎜ √ √ ⎜ 2 ⎜− 2 ⎝ 2 2 0 0

where matrix {aij } has the form: ⎞ 0⎟ ⎟ ⎟. 0⎟ ⎠ 1

We obtain: d15 = 2d131 = (d132 + d231 ) =

d14 + d25 = d14 2

so that d15 = d14 = 0.17 × 10−11 C N−1 . d31 = d311 = whence d31 =

d36 d312 + d321 = 2 2

d36 = 2.6 × 10−11 C N−1 . 2

482

Symmetry and Physical Properties of Crystals

Exercise 15.3 For group 422 (as well as for group 622), the form of the piezoelectric tensor, in the orthonormal axis system (Ox1 x2 x3 ) where Ox3 is parallel to the 4-fold axis (or the 6-fold axis) and Ox1 and Ox2 are parallel to the 2-fold axes, has the form: ⎞ ⎛ . . . . . d14 ⎝. . . . −d14 . ⎠ . . . . . . 0 We saw (Sect. 15.3.4) that the longitudinal piezoelectric surface is deﬁned by the set of points P such that the length of the vector OP, parallel to the direction of the unit vector s (s1 , s2 , s3 ), is given by si sj sk dijk (Eq. (15.25)). Here, the only coeﬃcients playing a part are d14 = d123 + d132 and d25 = d213 + d231 = −d14 . We ﬁnd: OP = s1 s2 s3 (d14 + d25 ) and, since d25 = −d14 , we have OP = 0. The longitudinal piezoelectric surface vanishes for all directions. Exercise 15.4 The form of the piezoelectric tensor, for group 32, in the orthonormal axis system (Ox1 x2 x3 ) deﬁned in the text, is: ⎞ ⎛ . . d11 −d11 . d14 ⎝ . . . . −d14 −2d11 ⎠ . . . . . . . 1. (a) In the orthonormal system (Ox1 x2 x3 ), rotated by angle θ with respect to (Ox1 x2 x3 ), the applied stress tensor has only one non-zero = T. component, T11 In the frame (Ox1 x2 x3 ), this tensor becomes: ⎛ ⎞ cos θ sin θ 0 cos2 θ ⎝ cos θ sin θ sin2 θ 0 ⎠ T. 0 0 0 We ﬁnd for the components of polarization P: ⎞ ⎛ ⎞ ⎛ d11 (cos2 θ − sin2 θ) d11 cos 2θ ⎠ T = ⎝ −d11 sin 2θ ⎠ T. −d11 sin 2θ P=⎝ 0 0 Its norm is: P = d11 T of θ.

cos2 2θ + sin2 2θ = d11 T . It is independent

(b) P encloses with direction Ox1 the angle ϕ such that ϕ = −2θ. Thus the polarization rotates twice as fast as the stress in the plane(Ox1 , Ox2 ), and in the opposite direction.

Chapter 20 – Solutions to the exercises

483

(c) From question (1a), we see that P will be parallel to Ox2 if cos 2θ = 0, hence when θ = π/4 + p π/2 with p an integer. It is therefore suﬃcient to apply a uniaxial stress at 45◦ to the axes Ox1 and Ox2 . 2.

We saw that d111 = si sj sk dijk (Eq. (15.25)), so that here: d111 = s1 d111 (s21 − 3s22 ). Neither d14 nor d25 = −d14 are involved, since the corresponding terms vanish. In spherical coordinates (θ, ϕ), we obtain: d111 = d111 sin3 θ(cos3 ϕ − 3 sin2 ϕ cos ϕ) = d111 sin3 θ cos 3ϕ. The intersection of this surface with the plane (Ox1 , Ox2 ) is obtained for θ = π/2 and d111 = d111 cos 3ϕ (Fig. 20.37, showing d111 /d111 ). The curve is periodic vs ϕ, with period 2π/3, in agreement with the presence of the 3-fold axis. x2 1

–1

0

1

x1

–1

Figure 20.37

Exercise 15.5 1.

The piezoelectric tensor for ⎛ . ⎝. .

group ¯43m is given by: ⎞ . . d14 . . . ⎠. . . . d14 . . . . d14

Due to the form of this tensor, we must apply T4 = T23 , or T5 = T13 , or T6 = T12 . 2.

Using (15.25):

d111 = si sj sk dijk = 3s1 s2 s3 d14

so that d111 = 3d14 cos θ sin2 θ cos ϕ sin ϕ =

3 d14 cos θ sin2 θ sin 2ϕ. 2

484 3.

Symmetry and Physical Properties of Crystals d111 is maximal for ϕ = π/4 + p π/2 (p an integer) and for

∂d111 = 0. ∂θ

3 3 ∂d111 = d14 sin 2ϕ sin θ(2 cos2 θ − sin2 θ) = d14 sin 2ϕ sin θ(3 cos2 θ − 1) ∂θ 2 2 which vanishes for sin θ = 0 so that θ = 0 or π but, for these values, d111 is zero, hence minimal. √ d111 is maximal for 3 cos2 θ −1 = 0, hence cos θ = 1/ 3, or θ = 54.7◦ . This value of θ, along with ϕ = 45◦ , are the spherical coordinates of direction [111] in the cube. 4.

In the orthonormal set of axes (Ox1 x2 x3 ) parallel to the basis vectors of the cubic unit cell, the only non-zero component of strain is S6 , with S6 = d14 E. The strain tensor can be written as: ⎞ ⎛ d14 E 0⎟ ⎜ 0 2 ⎟ ⎜d E . ⎜ 14 0 0⎟ ⎠ ⎝ 2 0 0 0 The relative volume variation is given by the trace of this tensor, hence ΔV = 0. V To determine the new shape of the solid, we express the tensor in a coordinate system where Ox1 is parallel to [110], Ox2 is parallel to [¯110] and Ox3 is unchanged. The transformation matrix from the referential (Ox1 x2 x3 ) to this frame is: √ ⎞ ⎛√ 2 2 0⎟ ⎜ 2 2 ⎟ ⎜ √ √ ⎟ ⎜ 2 ⎟. ⎜ 2 ⎜− 0⎟ ⎠ ⎝ 2 2 0 0 1 of the strain tensor in the frame (Ox x x ) are given The components Sij 1 2 3 by: Sij = aik ajl Skl . We obtain: = S31 = S32 = S12 = 0, S33

d41 E = 5 × 10−6 , 2 d41 E =− = −5 × 10−6 . 2

= S12 = S11 S22 = −S12

Exercise 15.6 ∞ m, with the ∞-order axis parallel to A uniaxial stress has symmetry group m the stress-producing force.

Chapter 20 – Solutions to the exercises

485

The polarization (with symmetry ∞m), if it exists, must be at least as sym∞ m. metric as the intersection of the crystal’s point group and of m ∞ 1. (a) The intersection of group 32 and of m (with the ∞ order axis m parallel to the 3-fold axis) is 32. No polarization can exist.

− mm

32

32

Figure 20.38

(b) The intersection is group 2, where the 2-fold axis is parallel to the uniaxial stress. This group is consistent with a polarization parallel to this 2-fold axis, and thus parallel to the applied stress.

P

32

Figure 20.39 (c) The intersection is again group 2, with the 2-fold axis perpendicular to the uniaxial stress. This group is consistent with a polarization parallel to the 2-fold axis, hence perpendicular to the applied stress.

32

P

Figure 20.40 (d) A shear stress T12 has symmetry group mmm, where two of the mirrors are at an angle of 45◦ to the axes Ox1 and Ox2 . The intersection of groups 32 and mmm is empty. A polarization can exist but, if it does, its direction cannot be predicted.

486

Symmetry and Physical Properties of Crystals

=

empty set

32

Figure 20.41 For ZnO, with point group 6mm: (a) Uniaxial stress parallel to Ox3 : the intersection of the symmetry groups of the crystal and of the stress is group 6mm. There can exist a polarization parallel to Ox3 .

− mm

6mm

6mm

Figure 20.42

6mm

(b) Uniaxial stress parallel to Ox1 : the intersection of the symmetry groups of the crystal and of the stress is group mm2. There can exist a polarization parallel to Ox3 .

2.

− mm

mm2

Figure 20.43 (c) The same result as in (b) is obtained for a uniaxial stress parallel to Ox2 .

Chapter 20 – Solutions to the exercises

487

Exercise 15.7 1.

The intersection of group ¯42m and of the group, mmm, of the shear stress in the conﬁguration of Figure 20.44a is group mm2. There can exist a polarization parallel to the 2-fold axis because mm2 is a subgroup of ∞m if the ∞-order axis is parallel to the 2-fold axis.

2.

The intersection of group ¯42m with the group mmm of the shear stress in the conﬁguration of Figure 20.44b leads to group 222, which is not a subgroup of ∞m. No polarization can exist.

(a)

=

=

– 42m

(b)

– 42m

Figure 20.44

20.14. Exercises for Chapter 16 Note: for clarity, the diﬀerence between ne and no is very much exaggerated in all ﬁgures. Exercise 16.1 The light ray is parallel to the normal to the index surface. For the ordinary ray, δ = 0. For the extraordinary ray, we draw the normal to the index surface at Pe , the intersection of the index surface and the wave vector starting at O. Let ϕ and θ be the angles of the normal to the index surface and the wavevector, respectively, with axis Ox2 .

488

Symmetry and Physical Properties of Crystals x3 no

Pe

k

Po

O

ne

x2

Figure 20.45 We have δ = ϕ−θ. The equation of the extraordinary index surface is given by: x22 x2 + 32 = 1. 2 ne no

The normal to this ellipsoid, at Pe (x2 , x3 ), has components:

2x2 2x3 , 2 n2e no

and

n2 n2 x3 n2e = e2 tan θ = v tan θ if we set v = e2 , 2 n o x2 no no tan ϕ − tan θ (v − 1) tan θ tan δ = tan(ϕ − θ) = = . 1 + tan ϕ tan θ 1 + v tan2 θ tan ϕ =

The maximum value of δ is obtained for: d(tan δ) (1 + tan2 θ)(v − 1) 1 − v tan2 θ = 0, = 2 2 dθ (1 + v tan θ) so that i)

(v − 1) = 0 → v = 1. This is the special trivial case where ne = no and δ = 0, the minimum value.

ii) 1 − v tan2 θ = 0 → tan2 θ = ne ≈ no .

1 n2 − n2o ne − no n2 ≈ if = o2 → tan δ = e v ne 2no ne ne

Numerically: for quartz, δ = 0.33◦ . Since no and ne are not very diﬀerent, the angle θ for which δ is maximal is not very diﬀerent from 45◦ . Exercise 16.2 The ordinary ray goes through the plate without being deviated. The extraordinary ray is parallel to the normal to the extraordinary index surface at Pe . The same approach as in the above exercise shows that the components of the normal to the index surface which are respectively parallel to Ox2 and Ox3 are 2x2 /n2e and 2x3 /n2o . Let ϕ and θ be the angles respectively enclosed with

Chapter 20 – Solutions to the exercises

489

axis Ox3 by the normal to the index surface and the wave-vector. tan ϕ = Since, at Pe , x3 = x2 , tan ϕ =

x2 n2o . n2e x3

n2o . n2e

Numerically: ϕ = 51.2◦ . The deviation δ between the ordinary and extraordinary rays is δ = ϕ − θ = 6.2◦ . In the plate, the extraordinary wave-vector is perpendicular to the plate (Descartes’ law at the entrance surface). At the exit of the plate, it remains normal to the plate. The shift Δ = e tan δ = 0.11 cm = 1.1 mm. x2 ne

P e no x3

Figure 20.46 Exercise 16.3 1.

At the entrance of the prism, the ordinary and extraordinary waves propagate with no deviation of either the wave-vector or the ray direction. The ordinary ray is polarized perpendicular to the optic axis, hence parallel to the edge of the prism. δo and δe are the deviations of the ordinary and extraordinary rays respectively. The incidence angle i on the exit surface is equal to 30◦ for both waves. Let ro and re be the refraction angles for the ordinary and extraordinary waves respectively. In air, the directions of the wave-vector and of the ray coincide. The deviations δo and δe of the ordinary and extraordinary rays are δo = ro − i and δe = re − i. Hence: ro = δo + i = 56.02◦ and re = δe + i = 48.01◦ . Applying Descartes’ laws yields no = 1.6585 and ne = 1.4865.

2.

At the prism entrance, the ordinary and extraordinary wave-vectors are not deviated (application of Descartes’ laws to the wave-vectors). The same applies to the ordinary ray, but the extraordinary ray propagates along the normal at Pe to the index surface. The incidence angle of the ordinary and extraordinary wave-vectors on the exit surface is i = 30◦ ,

490

Symmetry and Physical Properties of Crystals C

A

x3

Ro

B 9

30°

Pe

i

Re

i

x2 e

30°

9

B

x3

re

Re Ro

Pe O

C

30°

A

(a)

x2

(b)

Figure 20.47 and the application of Descartes’ laws (to the wave-vectors) provides the direction of the wave-vectors in air at the prism exit. This is also the direction of the rays. For the ordinary ray, we ﬁnd ro = 56.02◦ , and the deviation, as above, is δo = 26.02◦ . For the extraordinary ray, we must determine the value n of the extraordinary index, equal to the radius vector of the index surface at Pe . The coordinates of Pe are x3 = n sin θ and x2 = n cos θ with θ = 30◦ . The following relation must hold: n2 cos2 θ n2 sin2 θ + =1 n2e n2o

so that

n2 = 1/

cos2 θ sin2 θ + n2e n2o

.

We ﬁnd n = 1.5245. Thus: n sin i = sin re so that re = 49.66◦ and δe = 19.66◦ . Exercise 16.4 The incident beam goes through the ﬁrst prism undeviated. At the exit from this prism, the calcite-air interface can give rise to total reﬂection. For the ordinary ray, total reﬂection occurs for an angle of incidence on the interface equal to the angle θ of the prisms, such that no sin θ > 1, so that θ > 37.09◦ . For the extraordinary ray, total reﬂection occurs for an angle θ such that ne sin θ > 1, so that θ > 42.29◦ . Thus, for an angle θ such that 37.09◦ < θ < 42.29◦ , the ordinary ray is totally reﬂected and the extraordinary ray is transmitted by the prism, with its polarization in the plane deﬁned by the optic axis and the wave-vector. The polarization is perpendicular to the plane of the ﬁgure.

Chapter 20 – Solutions to the exercises

491

9

9

9

De

9

Figure 20.48 Exercise 16.5 1.

In a uniaxial material, the electrical induction vector D of the ordinary wave is perpendicular to the optic axis, hence in this case in the plane of the ﬁgure. For the extraordinary wave, D is perpendicular to the plane of the ﬁgure. D

A glass 30°

9

Do

De 30°

re

9

i’o

B

Re

r’o

30°

9

r’e

Ro

calcite C

Figure 20.49 2.

In the calcite prism, propagation occurs as in an isotropic material with an index no for the ordinary wave and an index ne for the extraordinary wave. The angle of incidence for each of these waves at the calcite-glass interface is i = 30◦ . Applying Descartes’ laws to this interface yields: i)

for the ordinary wave, no sin i = n sin ro where n is the index of the glass. We obtain: ro = 32.34◦ .

ii) for the extraordinary wave, ne sin i = n sin re , and re = 28.65◦ . At the glass–air interface, the angles of incidence are respectively io = 2.34◦ and ie = 1.35◦ . Descartes’ laws yield, for the refraction angles: ro = 3.63◦ and re = 2.09◦ , respectively. The deviation between the two outgoing beams is α = ro + re = 5.72◦ .

492

Symmetry and Physical Properties of Crystals

Exercise 16.6 The ordinary ray goes through both prisms undeviated. In the ﬁrst prism, the wave-vector is parallel to the optic axis, and the index is no irrespective of the polarization. In the second prism, the index surface intersects the plane of the ﬁgure along two circles, with radii no and ne . The polarization of the ordinary ray is normal to the optic axis, and that of the extraordinary ray is perpendicular to the plane of the ﬁgure. For the latter polarization, the index is no in the ﬁrst prism, and ne in the second one. At the interface between the two prisms, the angle of incidence i is 30◦ and the refraction angle re is given by no sin i = ne sin re . We obtain re = 33.9◦ . The wave-vector and the ray are parallel. The angle of incidence on the exit surface is 3.9◦ and the angle of refraction is equal to the angle α we are seeking. ne sin 3.9◦ = sin α. Thus α = 5.8◦ . A

9

D

30° Do

9 i

re

Do

Do

9

De

9

De

Ro Re

30° B

C

Figure 20.50

20.15. Exercises for Chapter 17 Exercise 17.1 1.

For normal incidence, the wave-vectors and the rays for both the ordinary and the extraordinary waves go through the plate without being deviated. The polarization of the ordinary ray is perpendicular to the optic axis, and we choose this direction as the Oy axis. That of the extraordinary ray is parallel to the plane of the ﬁgure, and this will be the direction of axis Ox.

2.

The phase shift ϕ between a wave polarized parallel to Oy and a wave polarized parallel to Ox is given by: ϕ=

2π(no − ne )e . λ

Chapter 20 – Solutions to the exercises

493

9

O

x

9 Eo

z

Ee

z

Figure 20.51 Since the crystal is positive, ϕ is negative for all values of e. The wave is a quarter-wave plate if ϕ = − π2 (1 + 2p), with p a positive integer, so that: e=

λ (1 + 2p). 4(ne − no )

Numerically, e = 16.4 μm + p(32.8) μm. If e = 16.4 μm, ϕ = −π/2; if e = 49.2 μm, ϕ = −3π/2, which is equivalent to + π/2. For a half-wave plate, ϕ = −π(1 + 2p), so that: e=

λ (1 + 2p). 2(ne − no )

Numerically, e = 32.8 μm + p(65.6) μm. 3.

After the quarter-wave plate, the electric ﬁeld is, in Jones notation; √ 2 E Ex = 2 √ √ 2 2 Ey = E exp(iϕ) = − i E 2 2 for ϕ = − π/2 (e = 16.4 μm). After the plate, the wave is right-circular polarized. A left-circular polarization would be obtained by rotating the plate through π/2 around the incident beam. The phase shift would then be +π/2. Another approach consists in turning the polarizer by π/2 around the incident beam, so that the polarization is in the second quadrant.

4.

The second quarter-wave plate contributes an additional phase shift by −π/2, so that: √ √

2 2 1 1 π = E E , −1 −ie−i 2 2 2

494

Symmetry and Physical Properties of Crystals a wave with linear polarization parallel to the second bisector direction. This result is no surprise since the two quarter-wave plates together form a half-wave plate.

5.

Natural light is unpolarized, and it can be described as the sum of two components with perpendicular linear polarizations, with a phase shift that varies randomly in time. A quarter-wave plate contributes an additional phase shift by π/2 to each of these phase shifts, which vary randomly as before. After the plate, light therefore remains unpolarized.

Exercise 17.2 1.

The neutral lines are respectively parallel and perpendicular to the optic axis. In the case of quartz, the ordinary polarization (perpendicular to the optic axis) corresponds to the fast line, and the extraordinary polarization to the slow line (parallel to the optic axis). We choose axes Ox and Oy respectively parallel to the fast and slow neutral lines. y (ne) A P

j

i

x (no)

Figure 20.52 2.

After the polarizer (Fig. 20.52), the electric ﬁeld in Jones notation is:

E 0 cos α . E 0 sin α After the plate, it becomes:

E 0 cos α E 0 eiϕ sin α

,

2π where ϕ = (ne − no )e is the phase shift introduced by the plate. We λ can write: E = Eo (cos α i + eiϕ sin α j). After the analyzer (angle α with axis Oy), the amplitude E of the electric ﬁeld is given by: E = Eo cos α sin α(eiϕ − 1). The intensity I is proportional to: |E|2 = E × E ∗ = Eo2

sin2 2α iϕ (e − 1)(e−iϕ − 1) 4

Chapter 20 – Solutions to the exercises so that:

3.

495

I = I0 sin2 2α sin2

ϕ . 2

ϕ If α = 45◦ , then I = I0 sin2 . 2 i) I = 0 corresponds to a phase shift ϕ = 2pπ (p an integer), i.e. either no plate, or a plate with thickness such that the phase shift is a multiple of 2π. ii) I is maximum for ϕ = π(1 + 2p), i.e. a half-wave plate: e=

4.

λ (1 + 2p) 2(ne − n0 )

emin =

and

λ . 2(ne − n0 )

e = 0.2 mm. The extinguished wavelengths are such that: ϕ = 2pπ = (ne − n0 )e

2π λ

λ=

so that

(ne − n0 )e . p

For p < 3 and p > 5, the wavelengths are not all in the visible range. p = 3: λ = 0.667 μm,

p = 4: λ = 0.5 μm,

p = 5: λ = 0.4 μm.

Exercise 17.3 1.

The components of the electric ﬁeld after the plate are: Ex = E cos ωt Ey = E cos(ωt + ϕ). To determine the curve drawn out by the end of vector E as t varies, we eliminate time between the expressions of Ex and Ey . We have: cos ωt =

Ex E

and

sin ωt = −

Ey cos ωt cos ϕ Ex cos ϕ − Ey + = E sin ϕ sin ϕ E sin ϕ

so that:

Ex2 (Ex cos ϕ − Ey )2 + =1 E2 E 2 sin2 ϕ which is the equation of an ellipse. After the plate, the wave is therefore elliptically polarized. To determine the directions of the axes of the ellipse, we express the equation of the ellipse in an axis system (OXY Z) rotated by an angle θ with respect to the neutral lines of the plate, and we seek the value of θ such that, in this new frame, the coeﬃcient of the crossed term (EX EY ) be zero. The calculation yields θ = 45◦ , whatever the value of ϕ. This result is valid only because the incident polarization is at 45◦ to the neutral lines of the plate. The axes of the ellipse are at 45◦ to the neutral lines of the plate, hence respectively parallel and perpendicular to the direction of the incident vibration.

496

Symmetry and Physical Properties of Crystals √

2.

√ 2 2 (EX −EY ) and Ey = (EX +EY ), and the equation Ex = If θ = 2 2 of the ellipse takes the form: 45◦ :

2 EY2 EX = 1. + 2E 2 cos2 ϕ/2 2E 2 sin2 ϕ/2

The ratio

B ϕ B of the ellipse axes has the value: = tan . A A 2

Exercise 17.4 If we rotate the plate, between crossed polarizer and analyzer, around the incident beam, which is perpendicular to the plate, extinction will occur when the neutral lines of the plate are respectively parallel to the polarization directions of the polarizer and the analyzer. Exercise 17.5 1.

The ordinary ray is refracted under

BY

G R E N O B L E

S C I E N C E S

Symmetry and Physical Properties of Crystals

C. Malgrange - C. Ricolleau - M. Schlenker

Symmetry and Physical Properties of Crystals

Grenoble Sciences The aim of Grenoble Sciences is twofold: – to produce works corresponding to a clearly defined project, without the constraints of trends nor curriculum, – to ensure the utmost scientific and pedagogic quality of the selected works: each project is selected by Grenoble Sciences with the help of anonymous referees. In order to optimize the work, the authors interact for a year (on average) with the members of a reading committee, whose names figure in the front pages of the work, which is then co-published with the most suitable publishing partner. Contact: Tel.: (33) 4 76 51 46 95 E-mail: [email protected] Website: https://grenoble-sciences.ujf-grenoble.fr Scientific Director of Grenoble Sciences Jean Bornarel, Emeritus Professor at the Joseph Fourier University, Grenoble, France Grenoble Sciences is a department of the Joseph Fourier University supported by the ministère de l’Enseignement supérieur et de la Recherche and the région Rhône-Alpes. Symmetry and Physical Properties of Crystals is an improved version of the original book Symétrie et propriétés physiques des cristaux by Cécile Malgrange, Christian Ricolleau and Françoise Lefaucheux, EDP Sciences, Savoirs Actuels Series, 2011, ISBN 978 2 7598 0499 3. The Reading Committee included the following members: – Ryszard Cach, Professor, University of Wrocław (Wrocław, Poland) – Vladimir E. Dmitrienko, Chief Researcher, A.V. Shubnikov Institute of Crystallography (Moscow, Russia) – José Goulon, Emeritus CNRS Senior Researcher, former group leader at the European Synchrotron Radiation Facility (Grenoble, France) – Hiroo Hashizume, Emeritus Professor, Tokyo Institute of Technology (Tokyo, Japan) – Jochen Schneider, Professor, former DESY Research Director (Hamburg, Germany), former director of the Experimental Facilities Division for the LCLS (Stanford, USA) Translation from original French version performed by Michel Schlenker; typesetting: Stéphanie Trine—special thanks to Konstantin Protassov and Alexei Voronine; figures: Sylvie Bordage, Alain Jeanne-Michaud; cover illustration: Alice Giraud, with sample of pyrite: mineral collection of Pierre and Marie Curie University, photograph Jean-Pierre Boisseau

Cécile Malgrange Christian Ricolleau Michel Schlenker •

Symmetry and Physical Properties of Crystals

123

Cécile Malgrange Université Pierre et Marie Curie Institut de Minéralogie, de Physique des Matériaux et de Cosmochimie case 115, 4 place Jussieu 75252 Paris cedex 05 France

Michel Schlenker Université Grenoble-Alpes Grenoble-INP et Institut Néel du CNRS B.P. 166 38042 Grenoble cedex France

Christian Ricolleau Université Paris Diderot-Paris 7 Laboratoire Matériaux et Phénomènes Quantiques Bâtiment Condorcet, case 7021 75205 Paris cedex 13 France Translated, revised and adapted from ‘‘Symétrie et Propriétés Physiques des Cristaux’’, Cécile Malgrange, Christian Ricolleau et Françoise Lefaucheux, EDP Sciences/CNRS Éditions 2011

ISBN 978-94-017-8992-9 DOI 10.1007/978-94-017-8993-6

ISBN 978-94-017-8993-6

(eBook)

Library of Congress Control Number: 2014944543 Springer Dordrecht Heidelberg New York London Ó Springer Science+Business Media Dordrecht 2014 This work is subject to copyright. All rights are reserved by the Publisher, whether the whole or part of the material is concerned, specifically the rights of translation, reprinting, reuse of illustrations, recitation, broadcasting, reproduction on microfilms or in any other physical way, and transmission or information storage and retrieval, electronic adaptation, computer software, or by similar or dissimilar methodology now known or hereafter developed. Exempted from this legal reservation are brief excerpts in connection with reviews or scholarly analysis or material supplied specifically for the purpose of being entered and executed on a computer system, for exclusive use by the purchaser of the work. Duplication of this publication or parts thereof is permitted only under the provisions of the Copyright Law of the Publisher’s location, in its current version, and permission for use must always be obtained from Springer. Permissions for use may be obtained through RightsLink at the Copyright Clearance Center. Violations are liable to prosecution under the respective Copyright Law. The use of general descriptive names, registered names, trademarks, service marks, etc. in this publication does not imply, even in the absence of a specific statement, that such names are exempt from the relevant protective laws and regulations and therefore free for general use. While the advice and information in this book are believed to be true and accurate at the date of publication, neither the authors nor the editors nor the publisher can accept any legal responsibility for any errors or omissions that may be made. The publisher makes no warranty, express or implied, with respect to the material contained herein. Printed on acid-free paper Springer is part of Springer Science+Business Media (www.springer.com)

In memory of Hubert Curien (1924–2005), Professor at Pierre & Marie Curie University, Paris, and member of the French Academy of Sciences. A great administrator, Minister of Research in the French government, he shared his enthusiasm for crystallography with his students through the courses he gave throughout his career.

Foreword Apart from amorphous bodies such as glasses, the arrangement of ions, atoms and molecules in solid matter is regular and presents properties of symmetry. Crystals present both translational and orientational properties of symmetry, which govern their physical properties. It is because of their triple periodicity that crystals grow with a regular habit: quartz prisms, diamond octahedra or garnet rhomb-dodecahedra, and that they present planar cleavage faces, those of the cube for rock-salt, and those of the rhombohedron for Iceland spar. It is this same periodicity that is at the origin of the band structure of solids and conditions the properties of materials used in microelectronics. It is thanks to the redundancy of the information provided by the diﬀraction in phase of X-rays, neutrons or electrons, by all the molecular groups repeated by the translations of a crystal that one can determine their atomic structure. If one wishes to ﬁnd the structure of a complex molecule such as a protein or a virus, one should therefore crystallize it. This is done systematically during the elaboration of drugs by the pharmaceutical industry. The orientational symmetry of crystals is present in all their properties, ﬁrst of all in their external shape. But it is often because a particular element of symmetry is absent that a property may exist. It is because hydrated ammonium tartrate has no centre of symmetry that it is optically active, which Louis Pasteur associated to its external shape, right or left, thus discovering chirality (1848). It is because of symmetry considerations that the Curie brothers, Jacques and Pierre, looked for, and found, piezoelectricity in 1880. If one cools barium titanate below 120◦ C, its structure is modiﬁed. Above, it is cubic holohedral, below, it is tetragonal, with as its only symmetry elements a four-fold axis and mirrors parallel to that axis. It is this symmetry which makes it possible for a spontaneous electric polarisation to appear, and for the crystal to become pyroand ferroelectric. Generally speaking, the properties associated to structural phase changes depend on the relations between symmetry groups and their subgroups. The description of the symmetry operations of crystals and of the resulting physical properties is the aim of the present book. These operations are part of a complex system which was not grasped at once. It was a long way from Aristotle’s elements to the concept of space lattice. The ancients were always fascinated by the regularity of six-sided prisms of rock-crystal, as noted by

VIII

Symmetry and Physical Properties of Crystals

Pliny the Elder in his Natural History (77 A.D.). Kepler (1611), followed by Descartes (1637) and Bartholin (1661) tried to interpret the formation of sixcornered snowﬂakes by the agglomeration of six spherules round a seventh one. Kepler was the ﬁrst to describe the primitive and face-centred cubic lattices and the hexagonal lattice, although he did not call them that way. Compact pile-ups were considered similarly by Hooke (1665) and Huygens (1678) to explain the shape of quartz and the cleavage rhombohedron of calcite, respectively. The constancy of interfacial angles was established in the seventeenth and the eighteenth centuries by Steno (1669), Carangeot (1780) and Romé de l’Isle (1783). At the end of the eighteenth century, Bergman (1773) for calcite and Haüy (1784) in a general way, showed that the external shape of crystal may be obtained by a regular and triply periodic pile-up of identical elemental parallelepipeds, now called unit cells, and called molécules intégrantes by Haüy. But Haüy confused the unit cell with its chemical content and did not accept the notion of isomorphism introduced by Mitscherlich (1819). His classiﬁcation of crystals was based on their geometrical shape while that of the German School, led by Weiss (1817), was based on systems of symmetry axes. Haüy’s main merit was nevertheless to have introduced the notion of three-dimensional periodicity which deﬁnes the crystalline medium and to have established the geometrical properties of lattice planes by means of the law of simple rational intercepts. The relations between symmetry and properties were established in steps all along the nineteenth century: the 7 crystal systems (Mohs, 1822), the notion of point lattice (Seeber, 1824), the 32 crystal classes (Frankenheim, 1826; Hessel, 1830), the notion of hemihedry (Delafosse, 1840), molecular chirality (Pasteur, 1848), the 14 Bravais lattices (1850), groups of motion including helicoidal motions, the 65 chiral groups (Sohncke 1865), and, ﬁnally, the 230 space groups (Fedorov, 1890; Schoenﬂies, 1891; Barlow, 1894).1 The description of physical properties in their geometrical form requires in general other mathematical tools, such as tensors, which were ﬁrst introduced in elasticity by Voigt (1899) and Brillouin (1949). If one pulls a rod made of an isotropic material, its length increases and its cross-section decreases. A scalar is insuﬃcient to describe the response of the material to an excitation and two constants are necessary to describe the resulting deformation. Similarly, the polarisation of an anisotropic dielectric can only be expressed by way of a tensor. The book by Cécile Malgrange, Christian Ricolleau and Michel Schlenker is an extended translation of a ﬁrst version in French by Cécile Malgrange, Christian Ricolleau and Françoise Lefaucheux. It comprises three parts of roughly equal importance: 1) a ﬁrst part on crystal symmetry, symmetry operations, crystal lattices, point groups and space groups; 2) a second part on crystal anisotropy and tensors applied to elasticity, propagation of elastic waves in crystals and piezoelectricity; 3) a third one on the optical properties of crystals, polariza1. A. Authier, Early Days of X-Ray Crystallography (Oxford University Press, Oxford, 2013)

Foreword

IX

tion, optical activity and electro-optical eﬀects. The various types of chemical bonds are also described in a small chapter between the ﬁrst and the second parts. Most chapters include an annex on a particular topic related to one of the points developed in the chapter, aimed at exciting the curiosity of the reader, and these complements are a real added value to the book. Exercises are also included, the solutions of which are given at the end of the book. They constitute a very valuable pedagogical tool. The whole of the book is written in a very clear and rigorous way. The publication of a new, up-to-date, textbook of crystallography and crystal physics will be very welcome at a time when crystallography courses are disappearing in most universities throughout the world, although these disciplines represent basic knowledge compulsory for anyone doing material science, Earth science, biochemistry, solid state physics or chemistry.

André Authier Professor Emeritus, Pierre & Marie Curie University, Paris Former President of the International Union of Crystallography Member of the German Academy of Sciences

Preface Crystallography constantly enjoys a new youth, thanks in particular to the spectacular progress in X-ray sources (synchrotron radiation from dedicated facilities and, very recently, free electron X-ray lasers), which make it possible to investigate an extremely broad range of materials. Its contribution is vital in many scientiﬁc and technological areas. It makes it possible, for example, to understand, and even to predict the properties of materials as diverse as high-Tc superconductors, high performance magnets, or biological materials such as proteins. The pharmaceutical industry invests large funds to set up data banks of structures, determined in the crystallized state, of molecules which could become medicines, in order to correlate their conﬁguration to their healing action. Crystallography also is very important in nanoscience, since some materials, when prepared in the form of nano-objects, take on crystal structures which do not exist in the bulk and which necessarily aﬀect their physical and chemical properties. Geophysicists obtain major information about the Earth mantle by investigating crystallized materials under extreme temperature and pressure conditions. In technology, we must mention structural wonders such as thin ﬁlm based artiﬁcial crystals (multilayers and superlattices) of semiconductors or magnetic materials. These have for several years been present in the giant or tunnel magnetoresistance read heads of the hard drives in all our computers. On the other hand, understanding the relation between the structure and the macroscopic properties of crystals opens the way to the use of physical properties with many applications. Thus piezoelectricity, i.e. the production of an electrical voltage under the eﬀect of stress, is the basis of our quartz watches and plays a central role in cell phones. Electro-optical eﬀects, the change in refractive indices under the eﬀect of an electric ﬁeld, entail a change in light propagation in materials. This book is mostly a translation of Symétrie et propriétés physiques des cristaux, published by EDP Sciences, Orsay, France in 2011. It provides the fundamentals underpinning all these research and application areas. In the ﬁrst part, it describes in a clear and thorough way the periodicity of crystals and their symmetry, both at the microscopic level (space groups) and at the macroscopic level (point groups). It includes a presentation of the crystallography of two-dimensional systems such as surfaces and interfaces.

XII

Symmetry and Physical Properties of Crystals

The second part is dedicated to various physical properties of crystals. They are described in the tensor formalism which is natural for them, emphasizing their link with crystal symmetry. We show in particular how a given property is allowed or forbidden by various crystal symmetries, and how the coeﬃcients of the characteristic tensor are related for the various point groups. We deal not only with basic properties such as elasticity and birefringence, but also with properties which are less often dealt with, such as piezoelectricity, optical activity or the electro-optical eﬀects. Each chapter starts with a short presentation of its contents, and almost all chapters are complemented by exercises through which the notions introduced can be concretely applied, and thus mastered. For these exercises to be a real studying tool, the solutions are explicitly given as a ﬁnal separate Chapter 20. Many of the chapters also include a brief complement, intended to give a glimpse into an area related to that of the chapter and to whet the reader’s scientiﬁc appetite, for example on how and what for crystals are grown, with what probes crystal structures can be determined, etc. This book originates in courses we gave at Paris Diderot University and at Grenoble Institute of Technology, France. It is aimed, with no special prerequisite, at students in crystallography, physics and engineering (especially materials science and electrical engineering) curricula, and at PhD students. It should also be a reference book for researchers and engineers involved, in their daily activity, in the properties of crystals. The authors sincerely thank the ﬁve members of the Advisory Editorial Committee for their very valuable suggestions, the vast majority of which were followed. They are also very grateful to Professor André Authier for writing the Foreword, which actually is a very informative chapter on the history of crystallography. The authors intend to correct the mistakes and typos which will, in spite of their eﬀorts, have remained in this ﬁrst edition. Errata sheets will be provided at https://grenoble-sciences.ujf-grenoble.fr/ouvrage/symmetry-crystals Comments from readers are very welcome. Please write to [email protected] Cécile Malgrange, Christian Ricolleau, Michel Schlenker.

Table of symbols a, b, c

Basis vectors of the unit cell in direct space

a, b, c

Lengths of the basis vectors of the unit cell in direct space

a∗ ,

b∗ ,

c∗

Basis vectors of the reciprocal unit cell

a∗ ,

b∗ ,

c∗

Lengths of the basis vectors of the reciprocal unit cell

v0

Volume of the direct unit cell

v0∗

Volume of the reciprocal unit cell

[uvw] < uvw >

Lattice row parallel to the vector ua + vb + wc Set of lattice rows equivalent to [uvw] through all the symmetry operations of the crystal group

(hkl)

Family of lattice planes with Miller indices h, k and l

(hkil)

Family of lattice planes with Miller indices h, k, i and l for a hexagonal lattice

{hkl}

Set of lattice planes equivalent to (hkl) through the symmetry operations of the crystal group

{hkil}

Set of lattice planes equivalent to (hkil) through the symmetry operations of the crystal group, for a hexagonal lattice

dhkl

Distance between two neighboring (hkl) lattice planes, i.e. the lattice spacing of family (hkl)

e 1 , e2 , e3

Basis vectors of an orthonormal frame

{Mij }

The matrix for which Mij is the coeﬃcient located on the i-th row and the j-th column

{aij } = A

Transition matrix for going over from an orthonormal frame to another one

V

Polar vector

V

Axial vector

[T ]

Tensor

Tij

Components, in a given orthonormal axis system, of a rank-2 tensor [T ]. The associated matrix is noted T .

Tijk

Components, in a given orthonormal axis system, of a rank-3 tensor [T ]

XIV

Symmetry and Physical Properties of Crystals

eij

Components of the tensor of displacement gradients, or distorsion tensor, [e]

T

The set of the crystal lattice translations

Gs

Space group

Gp

Point group

[S], Sij

Strain tensor, and its components

[T ], Tij

Stress tensor, and its components

Sα , Tα

Contracted notation (Voigt’s notation) for the tensors [S] and [T ]. α ranges from 1 to 6, so that the components of these tensors form column vectors with 6 rows.

[s], sijkl

Compliance tensor, and its components

[c], cijkl

Stiﬀness tensor, and its components

Θ

Temperature

S

Entropy

E

Electric ﬁeld

D

Electric induction

P

Polarization

[ε], εij ε0 [η], ηij

Relative permittivity (or dielectric constant) tensor, and its components Permittivity (or dielectric constant) of vacuum Electric impermeability tensor, and its components

δij

Kronecker symbol

δijk

Levi-Civita, or permutation, tensor

[G], Gij

Gyration tensor, and its components

[d], dijk

Piezoelectric tensor, and its components

[r], rijk

Linear electro-optic tensor, or Pockels tensor, and its components

[z], zijkl

Quadratic electro-optic tensor, or Kerr tensor, and its components

[p], pijkl

Elasto-optic tensor and its components

[π], πijkl

Piezo-optic tensor and its components

Contents Chapter 1 – Introduction 1.1. Crystal order ..................................................................... 1.2. Order on a macroscopic scale ................................................ 1.3. Order on a microscopic scale ................................................ 1.4. Basic assumptions of geometrical crystallography ..................... 1.5. Anisotropy of physical properties .......................................... 1.6. Remarks on the scope of this book : topics left out ................... Complement 1C. Crystal growth .................................................... 1C.1. Natural growth of single crystals ................................. 1C.2. Crystal growth for scientiﬁc purposes ........................... 1C.3. Industrial crystal growth ........................................... 1C.4. Growth of single-crystal thin ﬁlms ............................... Further reading .................................................................. References .................................................................................

1 1 3 4 6 6 7 8 8 8 9 10 10 11

Chapter 2 – Symmetry operations 2.1. Isometries ......................................................................... 2.2. Symmetry operations. Symmetry elements .............................. 2.2.1. n-fold rotations and axes ........................................... 2.2.2. n-fold rotoinversions and n-fold rotoinversion axes, denoted as n ¯ -fold axes .............................................. 2.2.3. Translations ............................................................ 2.2.4. Screw axes and glide mirrors ...................................... 2.2.5. Note ...................................................................... 2.3. Introduction to symmetry groups .......................................... 2.4. Exercises ..........................................................................

13 13 14 14

Chapter 3 – Crystal lattices 3.1. Direct lattice ..................................................................... 3.1.1. Unit cell, row .......................................................... 3.1.2. Lattice planes .........................................................

23 23 23 28

15 16 17 18 18 20

XVI

Symmetry and Physical Properties of Crystals

3.1.3. Wigner-Seitz cell ...................................................... Reciprocal lattice ............................................................... 3.2.1. Introduction based on diﬀraction ................................ 3.2.2. Alternative deﬁnition of the reciprocal lattice ................ 3.2.3. Properties of the reciprocal lattice ............................... 3.2.4. Crystallographic calculations ...................................... 3.3. Properties of crystal lattices ................................................. 3.3.1. Centers of symmetry ................................................ 3.3.2. n-fold and n ¯ -fold axes consistent with the crystalline state 3.3.3. The direct lattice and the reciprocal lattice have the same symmetry elements ...................................... 3.3.4. Geometrical relation between the symmetry axes and the crystal lattice ............................................... 3.3.5. The lattice is at least as symmetrical as the crystal ........ 3.4. Crystal systems ................................................................. 3.4.1. Two-dimensional crystal systems ................................. 3.4.2. Three-dimensional crystal systems ............................... 3.5. Examples of reciprocal lattices .............................................. 3.5.1. Monoclinic lattice .................................................... 3.5.2. Orthorhombic, tetragonal and cubic lattices .................. 3.6. Hexagonal lattice and rhombohedral lattice ............................. 3.6.1. Hexagonal lattice ..................................................... 3.6.2. Rhombohedral lattice ............................................... 3.7. Bravais lattices .................................................................. 3.7.1. Why they are needed ................................................ 3.7.2. The fourteen Bravais lattices ...................................... 3.7.3. Reciprocal lattices of the non-primitive lattices .............. 3.8. Surface crystal lattice ......................................................... 3.8.1. Cut surface ............................................................. 3.8.2. Real surface ............................................................ 3.8.3. Notations ............................................................... 3.8.4. Reciprocal lattice ..................................................... 3.9. Exercises .......................................................................... Appendix 3A. The metric tensor ................................................... 3A.1. Deﬁnition ............................................................... 3A.2. Volume of the unit cell .............................................. 3A.3. Product of the matrices associated to the direct and reciprocal metric tensors ...................................... 3A.4. Calculation of lattice distances ................................... 3A.5. Applications ............................................................ 3.2.

32 32 32 34 35 37 40 40 40 41 42 43 43 43 44 47 47 47 48 48 48 50 50 52 53 54 55 55 56 58 59 63 63 63 64 65 65

Contents Chapter 4 – Relationship between space groups and point groups 4.1. Introduction ...................................................................... 4.2. Symmetry operations of the crystal ....................................... 4.2.1. Change in origin ...................................................... 4.2.2. The operations (S, t) form a group .............................. 4.2.3. The lattice translations form an invariant subgroup of the group of symmetry operations of the crystal ......... 4.3. Space groups and point groups ............................................. 4.4. Exercises .......................................................................... Complement 4C. Probes used for crystal structure determination ......... 4C.1. Possible probes and criteria for choice .......................... 4C.2. X-rays .................................................................... 4C.3. Neutrons ................................................................ 4C.4. Electrons ................................................................ Further reading .................................................................. Appendix 4A. General features of groups ........................................

XVII

67 67 70 70 71 72 73 75 76 76 76 78 79 79 80

Chapter 5 – Point groups 83 5.1. Introduction ...................................................................... 83 5.2. Stereographic projection ...................................................... 84 5.2.1. Deﬁnition ............................................................... 84 5.2.2. Examples ............................................................... 86 5.2.3. Application to rotoinversion axes or n ¯ -fold axes ............. 88 5.2.4. Family of equivalent directions ................................... 89 5.3. Improper groups ................................................................ 89 5.3.1. Preliminary remark .................................................. 89 5.3.2. Properties of improper groups .................................... 90 5.4. Enumeration of the proper point groups ................................. 91 5.4.1. Preamble ................................................................ 91 5.4.2. Groups containing only the symmetry operations associated to an axis An (cyclic groups) ....................... 92 5.4.3. Groups containing the symmetry operations associated to an axis An and to a perpendicular axis A2 , or dihedral groups .................................................... 92 5.4.4. Cubic proper groups ................................................. 93 5.5. Enumeration of the improper point groups .............................. 94 5.5.1. Improper groups containing inversion ........................... 94 5.5.2. Improper groups which do not feature inversion ............. 97 5.6. Classiﬁcation of the point groups .......................................... 101

XVIII

Symmetry and Physical Properties of Crystals

5.7. Laue classes ...................................................................... 5.8. Plane point groups ............................................................. 5.9. Isotropy point groups .......................................................... 5.10. Exercises .......................................................................... Appendix 5A. Complements on the stereographic projection ............... 5A.1. Stereographic projection of the transform of a given direction through the symmetry operations associated to various symmetry elements .................................... 5A.2. Stereographic projections of the symmetry elements of a cube ................................................................

106 107 107 109 111

111 112

Chapter 6 – Bravais lattices 6.1. Introduction ...................................................................... 6.2. Plane lattices .................................................................... 6.2.1. Group 1 ................................................................. 6.2.2. Group 3 ................................................................. 6.2.3. Group 4 ................................................................. 6.2.4. Group m ................................................................ 6.2.5. Conclusion .............................................................. 6.3. 3-dimensional lattices .......................................................... 6.3.1. Group 1 ................................................................. 6.3.2. Group 2 ................................................................. 6.3.3. Group 3 ................................................................. 6.3.4. Group 4 ................................................................. 6.3.5. Group 222 .............................................................. 6.3.6. Group 23 ................................................................

117 117 118 118 118 119 119 120 120 120 120 122 124 126 127

Chapter 7 – Space groups 7.1. Introduction ...................................................................... 7.2. Enumeration of the operations (S, t) ...................................... 7.2.1. S is a rotation. Deﬁnition of screw axes ........................ ¯ Deﬁnition of glide mirrors .. 7.2.2. S is a rotoinversion, noted S. 7.2.3. Product of a symmetry operation and a translation ........ 7.3. Enumeration of space groups ................................................ 7.3.1. Symmorphic space groups .......................................... 7.3.2. Non-symmorphic space groups .................................... 7.3.3. International Tables for Crystallography ....................... 7.4. Nomenclature .................................................................... 7.5. Examples: space groups of some structures ............................. 7.5.1. TiO2 -type structure (rutile) .......................................

129 129 130 131 134 136 139 139 142 146 149 151 151

Contents

XIX

7.5.2. Metals with close-packed hexagonal structure ................ 7.5.3. Structure of diamond ................................................ 7.6. Exercises .......................................................................... Complement 7C. Structure determination: outline ............................ Further reading .................................................................. References .................................................................................

152 154 155 158 161 162

Chapter 8 – Chemical bonds and crystal structures 8.1. Introduction ...................................................................... 8.2. Ionic bonds ....................................................................... 8.2.1. Nature and properties ............................................... 8.2.2. Bonding energy ....................................................... 8.2.3. Ionic structures with formula AX ................................ 8.2.4. Other cubic structures .............................................. 8.3. Covalent bonds .................................................................. 8.3.1. Nature of covalent bonds ........................................... 8.3.2. Basic property ......................................................... 8.3.3. Examples ............................................................... 8.3.4. Conclusion .............................................................. 8.4. Van der Waals bonds, or molecular bonds ............................... 8.4.1. Nature and properties ............................................... 8.4.2. Example ................................................................ 8.5. Metallic bonds ................................................................... 8.5.1. Nature and properties ............................................... 8.5.2. Examples ............................................................... 8.6. Remarks and conclusions ..................................................... 8.7. Exercises .......................................................................... Complement 8C. Magnetic structures ............................................. Further reading .................................................................. References .................................................................................

163 163 165 165 168 169 171 173 173 174 174 176 177 177 177 178 178 178 180 181 183 185 186

Chapter 9 – Crystal anisotropy and tensors 9.1. Introduction ...................................................................... 9.2. Anisotropic continuous medium ............................................ 9.3. Representing a physical quantity by a tensor ........................... 9.3.1. Example: electrical conductivity ................................. 9.3.2. A refresher on orthonormal frame changes .................... 9.3.3. Application to electrical conductivity ........................... 9.4. Tensors ............................................................................ 9.4.1. Deﬁnition of a tensor ................................................

187 187 188 189 189 191 193 194 194

XX

Symmetry and Physical Properties of Crystals

9.4.2. An important property ............................................. 9.4.3. Field tensors and material tensors ............................... 9.5. Symmetry properties of tensors ............................................. 9.5.1. Internal symmetry. Symmetric and antisymmetric tensors 9.5.2. External symmetry of material tensors. Curie’s and Neumann’s principles ................................ 9.6. Reduction in the number of independent coeﬃcients of a material tensor ............................................................ 9.6.1. Method using the transformation matrix ...................... 9.6.2. “Direct inspection” method ........................................ 9.6.3. Special case: central symmetry (inversion symmetry) ...... 9.7. Exercises .......................................................................... References ................................................................................. Chapter 10 – Second-rank tensors 10.1. Introduction ...................................................................... 10.1.1. Symmetric and antisymmetric tensors .......................... 10.1.2. Matrix form of second-rank tensors ............................. 10.1.3. Trace ..................................................................... 10.2. Representative quadric for a symmetric rank-2 tensor ............... 10.2.1. Characteristic surface ............................................... 10.2.2. Principal axes and principal coeﬃcients ........................ 10.2.3. Shape of the quadric ................................................. 10.3. Properties of the quadric ..................................................... 10.3.1. Normal to the quadric .............................................. 10.3.2. Length and physical meaning of the radius vector .......... 10.3.3. Intensity of a physical property in a given direction ........ 10.4. Geometrical determination of the principal axes and principal coeﬃcients: the Mohr circle construction ................................ 10.5. Eﬀect of crystal symmetry ................................................... 10.5.1. Triclinic system ....................................................... 10.5.2. Monoclinic system .................................................... 10.5.3. Orthorhombic system ............................................... 10.5.4. Uniaxial systems: rhombohedral, trigonal and hexagonal . 10.5.5. Cubic system .......................................................... 10.6. Axial vectors, or antisymmetric rank-2 tensors ......................... 10.6.1. Polar vectors, axial vectors ........................................ 10.6.2. Example of an axial vector: the cross product ............... 10.7. Exercises ..........................................................................

195 196 197 197 197 200 200 201 202 203 204 205 205 205 206 206 207 207 207 209 210 210 211 211 213 215 216 216 216 217 217 218 218 220 222

Contents

XXI

Chapter 11 – The stress tensor 11.1. Introduction ...................................................................... 11.2. Stress tensor ..................................................................... 11.2.1. Introduction ........................................................... 11.2.2. Deﬁnition of the stress tensor ..................................... 11.2.3. Normal stress and shear stress .................................... 11.3. Basic relation .................................................................... 11.4. Symmetry of the stress tensor ............................................... 11.5. Examples of stress tensors ................................................... 11.5.1. Uniaxial stress ......................................................... 11.5.2. Pure shear .............................................................. 11.5.3. Hydrostatic pressure ................................................. 11.6. Eﬀect of gravity ................................................................. 11.7. Exercises .......................................................................... References .................................................................................

225 225 225 225 227 229 230 233 234 234 235 235 236 238 240

Chapter 12 – Deformation of a solid. The strain tensor 12.1. Distortion tensor (displacement gradient tensor) ...................... 12.1.1. Deﬁnition ............................................................... 12.1.2. Physical meaning of components eij ............................ 12.2. Decomposition of the distortion tensor into a rotation and a strain .................................................. 12.2.1. Introduction using a simple example ............................ 12.2.2. Expressing the distortion associated to small rotations .... 12.2.3. Strain tensor ........................................................... 12.3. Elongation in a given direction ............................................. 12.4. Volume expansion (volumetric strain) .................................... 12.5. Special cases of strain ......................................................... 12.5.1. Simple elongation .................................................... 12.5.2. Pure shear strain ..................................................... 12.5.3. Simple shear strain ................................................... 12.6. Thermal expansion ............................................................. 12.7. Exercises ..........................................................................

241 241 241 243

Chapter 13 – Elasticity 13.1. Introduction ...................................................................... 13.2. Compliance and stiﬀness tensors ........................................... 13.2.1. Generalized Hooke’s law ............................................ 13.2.2. Symmetry of the compliance and stiﬀness tensors ...........

259 259 262 262 263

244 244 245 246 247 248 249 249 249 250 250 254

XXII

Symmetry and Physical Properties of Crystals

13.3. Contracted notation (Voigt’s notation) ................................... 13.3.1. Stress tensor ........................................................... 13.3.2. Strain tensor ........................................................... 13.3.3. Compliance tensor and stiﬀness tensor ......................... 13.3.4. Relation between the compliance and stiﬀness tensors ..... 13.4. Energy of a strained solid .................................................... 13.5. Eﬀect of crystal symmetry on the form of the elastic tensor ........ 13.5.1. Center of symmetry .................................................. 13.5.2. Groups 2, m and 2/m ............................................... 13.5.3. Groups 222, mmm and mm2 ...................................... 13.5.4. Groups 422, 4mm and 4/m mm .................................. 13.5.5. Cubic system .......................................................... 13.6. Isotropic materials .............................................................. 13.6.1. Expressing components sαβ as a function of E and ν ...... 13.6.2. Stiﬀness components. Lamé coeﬃcients ........................ 13.7. Representative surface for Young’s modulus ............................ 13.8. Compressibility .................................................................. 13.8.1. Bulk compressibility ................................................. 13.8.2. Linear compressibility of a bar .................................... 13.9. Notes on non-uniform stresses and strains ............................... 13.10. Exercises .......................................................................... Complement 13C. Plastic deformation and crystal defects .................. Further reading .................................................................. References .................................................................................

264 264 265 265 268 268 271 274 274 274 275 276 276 278 279 279 281 281 282 283 285 288 290 291

Chapter 14 – Elastic waves in crystals 14.1. Introduction ...................................................................... 14.2. Plane elastic waves ............................................................. 14.3. Application to a cubic crystal ............................................... 14.3.1. Propagation of a plane wave along direction [100] ........... 14.3.2. Propagation along direction [110] ................................ 14.4. Isotropic solid case ............................................................. 14.5. Microscopic approach – Crystal lattice dynamics ...................... 14.5.1. Linear chain of identical atoms ................................... 14.5.2. Linear chain with two diﬀerent atoms .......................... 14.5.3. Extension to the real crystal case ................................ 14.6. Exercises ..........................................................................

293 293 294 297 298 299 300 301 301 305 308 309

Contents

XXIII

Chapter 15 – Crystal thermodynamics. Piezoelectricity 15.1. Crystal thermodynamics ...................................................... 15.1.1. Conjugate variables .................................................. 15.1.2. Independent variables ............................................... 15.1.3. Principal eﬀects vs crossed eﬀects ............................... 15.1.4. Summary of the various eﬀects ................................... 15.1.5. Condensed representation of the physical property matrix 15.2. Pyroelectricity. Pyroelectric crystals ...................................... 15.3. Piezoelectric crystals ........................................................... 15.3.1. Direct eﬀect and inverse eﬀect .................................... 15.3.2. Piezoelectric tensor [d] and its two-subscript notation ..... 15.3.3. Eﬀect of crystal symmetry on the form of the tensor ....... 15.3.4. Longitudinal piezoelectricity surface ............................ 15.3.5. Other forms of piezoelectric coeﬃcients ........................ 15.3.6. Applications ........................................................... 15.4. Principal and crossed eﬀects under various conditions ............... 15.5. Exercises .......................................................................... Complement 15C. Electrostriction and magnetostriction .................... Further reading .................................................................. References .................................................................................

311 312 312 314 317 318 320 321 322 322 323 324 328 329 331 332 334 337 338 339

Chapter 16 – Light propagation in crystals 16.1. Maxwell’s equations ............................................................ 16.2. Light propagation in an isotropic material .............................. 16.3. Sinusoidal waves that are solutions of Maxwell’s equations ......... 16.4. Plane monochromatic wave in an anisotropic material ............... 16.4.1. Basic equation ......................................................... 16.4.2. Birefringence ........................................................... 16.4.3. Index surface .......................................................... 16.4.4. Index ellipsoid ......................................................... 16.4.5. Determining the induction vectors ............................... 16.4.6. Direction of energy propagation .................................. 16.5. Refraction of a plane wave at the boundary between two materials 16.5.1. The wave-vectors follow the Snell-Descartes law ............. 16.5.2. Application to uniaxial materials ................................ 16.6. Conclusion ........................................................................ 16.7. Exercises ..........................................................................

341 341 342 343 345 345 346 347 349 350 353 354 354 357 358 360

XXIV

Symmetry and Physical Properties of Crystals

Appendix 16A. Wave surface (or ray surface) and Huygens’ construction 364 16A.1. Wave surface (or ray surface) .................................... 364 16A.2. Huygens’ construction ............................................. 367 Chapter 17 – Polarization of light by crystals 17.1. Polarization state of an electromagnetic wave .......................... 17.1.1. Linearly polarized wave ............................................. 17.1.2. Circularly polarized wave .......................................... 17.1.3. Elliptically polarized wave ......................................... 17.1.4. Natural light ........................................................... 17.2. Jones notation ................................................................... 17.3. Linear polarizers ................................................................ 17.4. Phase-shifting plates ........................................................... 17.4.1. Half-wave plates ...................................................... 17.4.2. Quarter-wave plates ................................................. 17.5. Partially polarized waves and Stokes parameters ...................... 17.6. Exercises .......................................................................... References .................................................................................

369 369 370 370 372 372 373 374 376 377 378 379 382 384

Chapter 18 – Rotatory power and optical activity 18.1. Deﬁnition of the rotatory power of a material .......................... 18.2. Fresnel’s interpretation ........................................................ 18.3. Interpretation of rotatory power through the inﬂuence of the local environment ...................................................... 18.3.1. Eﬀect of spatial dispersion ......................................... 18.3.2. Wave propagation in optically active crystals ................ 18.4. Eﬀect of crystal symmetry on the gyrotropy tensor ................... 18.4.1. Centrosymmetric groups ............................................ 18.4.2. Non-centrosymmetric groups ...................................... 18.5. Rotatory power and chirality ................................................ 18.6. Absorption and conclusion ................................................... Complement 18C. Magnetic optical rotation .................................... Further reading .................................................................. Appendix 18A. Axial tensors, or pseudo-tensors ............................... 18A.1. Deﬁnition of axial tensors, or pseudo-tensors ................. 18A.2. Levi-Civita tensor, or permutation tensor ...................... 18A.3. The gyrotropy tensor [G] is a rank-2 axial tensor ............ 18A.4. Relation between tensors [G] and [β] ............................ References .................................................................................

385 385 386 388 388 390 393 393 394 396 400 401 402 403 403 403 404 405 406

Contents

XXV

Chapter 19 – Electro-optical and elasto-optical eﬀects 19.1. Introduction ...................................................................... 19.2. Electro-optical eﬀects .......................................................... 19.2.1. Linear electro-optical eﬀect, or Pockels eﬀect ................. 19.2.2. Applications of the linear electro-optical eﬀect ............... 19.2.3. Quadratic electro-optical eﬀect, or Kerr eﬀect ................ 19.3. Elasto-optical eﬀects ........................................................... 19.3.1. Deﬁnition ............................................................... 19.3.2. Application to the acousto-optical eﬀects ...................... 19.4. Exercises .......................................................................... Complement 19C. Frequency doubling, or Second Harmonic Generation Further reading ..................................................................

407 407 408 408 415 420 424 424 427 430 433 434

Chapter 20 – Solutions to the exercises 20.1. Exercises for Chapter 2 ....................................................... 20.2. Exercises for Chapter 3 ....................................................... 20.3. Exercises for Chapter 4 ....................................................... 20.4. Exercises for Chapter 5 ....................................................... 20.5. Exercises for Chapter 7 ....................................................... 20.6. Exercises for Chapter 8 ....................................................... 20.7. Exercises for Chapter 9 ....................................................... 20.8. Exercises for Chapter 10 ...................................................... 20.9. Exercises for Chapter 11 ...................................................... 20.10. Exercises for Chapter 12 ...................................................... 20.11. Exercises for Chapter 13 ...................................................... 20.12. Exercises for Chapter 14 ...................................................... 20.13. Exercises for Chapter 15 ...................................................... 20.14. Exercises for Chapter 16 ...................................................... 20.15. Exercises for Chapter 17 ...................................................... 20.16. Exercises for Chapter 19 ......................................................

435 435 436 444 445 450 456 458 459 461 463 470 475 479 487 492 499

General references

507

Index

511

Chapter 1

Introduction This chapter introduces the spatial periodicity and the macroscopic scale symmetry properties which characterize crystals.

1.1. Crystal order Depending on temperature and pressure, all materials take on three diﬀerent states: solid (S), liquid (L) and gas (G) (Fig. 1.1). However, when looking at matter from a microscopic point of view, there are only two really distinct states: the ordered state (grey area on Fig. 1.1) and the disordered state. It is clear that a gas at low pressure, consisting of a set of molecules separated by distances that are large compared to their size, is totally disordered. In a liquid, the molecules are in contact with one another, like marbles packed in a bag. A liquid is not completely disordered: there is some order, but only at short range. Furthermore, it is possible to go continuously from the gas state to the liquid state. At a temperature Θ between the temperature ΘT of the triple point and that ΘC of the critical point, a gas undergoing compression goes from the gas state (A) to the liquid state (B) through a sharp transition, liquefaction or condensation. But it is possible to go from A to B around the critical point, for instance by going from A to D at constant pressure, then from D to F at constant temperature, and then from F to B at constant pressure. In contrast, it is impossible to go from the disordered area to the ordered area without crossing the line, shown as a thick line on the ﬁgure, that clearly separates the ordered and the disordered domains. This line consists of two parts: one corresponds to sublimation (solid–gas transition) and to condensation for the inverse transformation, the other to melting (solid–liquid transition) and to solidiﬁcation for the inverse transformation. The equilibrium diagram of Figure 1.1 applies to most solids and their transition to a disordered state, either liquid or gas. However, for some solids, the liquid–solid transition is not sharp but continuous: this is the case for amorphous or glassy solids. When the temperature of such a material in liquid form is lowered, its viscosity increases, which means that its ﬂow is more and

© Springer Science+Business Media Dordrecht 2014 C. Malgrange et al., Symmetry and Physical Properties of Crystals, DOI 10.1007/978-94-017-8993-6_1

1

2

Symmetry and Physical Properties of Crystals p

melting curve ordered state

disordered state

S

B

F C

G L T

A

D

sublimation curve T

C

T

Figure 1.1: Equilibrium diagram for a pure substance, in a representation where pressure p is shown as a function of temperature T more diﬃcult. It forms a kind of paste, which ends up being solid but with a structure hardly more ordered than that of a liquid: it is a kind of set liquid – which corresponds to a metastable state. This book deals only with crystalline solids, characterized by long-range order. The size of the ordered regions depends on the conditions in which crystallization occurs. If no special care is exercised when solidifying a pure liquid, microcrystals appear at various points of the liquid, grow and end up being contiguous. Each small crystal is perfectly ordered, but there is no reason for these crystals to have the same orientation. We get a polycrystal, i.e. a solid made up of small crystals (grains) with the same structure, but diﬀerently oriented. This is the most prevalent case for materials and in particular for metals (Fig. 1.2). However, some minerals occur in single crystal form, i.e. in a form where the solid is identically oriented over its entire volume. This is the case for the gems of jewelers, and for some beautiful minerals which can be found in private or public collections1 (Fig. 1.3a). On the other hand, some crystals can be manufactured in the form of quite large single crystals. This is the case for silicon or quartz, which are produced as single crystals several tens of centimeters in size (Fig. 1.3b).

1. All museums of natural history have a section on minerals. If you visit Paris (France), you will enjoy in particular the mineral collection of Pierre & Marie Curie University (UPMC) and of the Institut de Minéralogie et de Physique des Milieux Condensés (IMPMC), located at 4 place Jussieu, in the 5th district (arrondissement).

Chapter 1 – Introduction

3

Figure 1.2: Scanning Electron Microscopy (SEM) image of the surface of a polycrystalline copper sample (courtesy Cyril Langlois)

(a)

5 cm

(b)

5 cm

Figure 1.3: (a) A sample of pyrite (iron sulﬁde, FeS2 ), mineral collection of Pierre & Marie Curie University (Paris 6) (photograph by Jean-Pierre Boisseau); (b) two bars of single crystal synthetic quartz produced by the SICN company (photograph by Alain Jeanne-Michaud)

1.2. Order on a macroscopic scale The existence of crystal order was sensed in the 17th century at the macroscopic scale, and recognized at the beginning of the 20th century at the microscopic scale. For instance, Niels Stensen, or Nicolaus Stenonius, or Steno, a Dane, noticed as early as 1669 that the angles between faces of natural crystals of quartz and some other minerals have a well deﬁned, constant value, independent of their origin. He then spelled out the law of constancy of angles, which was to be generalized to all crystals by Romé de l’Isle in 1783. This constancy of angles also shows up on the small crystals which form naturally during solidiﬁcation. The mineralogist René Just Haüy showed in 1784 how this regularity in angles can be explained. He had noticed that, when he would cleave2 a crystal of calcite, he would obtain smaller and smaller rhombohedra, all with the same 2. When a crystal of calcite is broken, the fracture surface features perfectly plane areas, with a restricted number of orientations. If one attempts, using a cutting tool and a small hammer, to cleave the crystal, i.e. to break it along one of these special areas, one obtains, provided the blade is properly oriented and the experimentalist has some experience, two fragments separated by a beautiful plane suface known as a cleavage surface.

4

Symmetry and Physical Properties of Crystals

angles. He then imagined that a ﬁnal stage, i.e. a small elementary rhombohedron which can no more be cut, should eventually be reached. He deduced that the macroscopic crystal should be formed from the regular stacking of small rhombohedra, all identical to this elementary rhombohedron which he called the “integrating molecule”. He then showed, and this is the strong point of his theory, that he could reconstruct all external forms of crystals by stacking identical elementary parallepiped-shaped blocks into successive layers which he shifted by a constant, integral number of units at each layer (Fig. 1.4). The parameters deﬁning the basic parallelepiped were characteristic of the crystal. The notions of periodicity and of crystal unit cell, which we will deﬁne later, thus appear.

Figure 1.4: A stacking of layers of identical parallelepipeds, regularly shifted to reproduce the actual habit of the crystal

1.3. Order on a microscopic scale After Haüy and until 1912 the concepts of symmetry and of internal periodicity in the crystal developed. However it was not evident, or at any rate not proved, that this internal order, viz. a triply periodic stacking, could exist in materials with any external shape. It was in fact through the discovery of X-ray diﬀraction by Max von Laue in 1912, and thanks to the work of William and Lawrence Bragg, that the existence of a periodic stacking of atoms in solids, as predicted by Haüy, could be evidenced. They showed that X-rays are diﬀracted by crystals along special directions, forming a discrete set of spots which could be interpreted only

Chapter 1 – Introduction

5

through a triply periodic stacking of the atoms. Thus crystalline solids can be represented using a crystal motif,3 comprising a ﬁnite number of atoms, periodically repeated along three non-coplanar directions with periods along these directions respectively a, b and c. Let us discuss a few examples to illustrate this notion of periodicity. Figure 1.5 shows a frieze formed by repeating, with period a, a motif. Figure 1.6 shows a sample of wallpaper featuring periodicity in two directions (periods a and b).

a

Figure 1.5: A decorative pattern from Arabic art, after J. Bourgoin, Arabic Geometrical Pattern and Design (Dover Publications, New York, 1973)

b a

Figure 1.6: A sample of wallpaper A crystal is thus formed from a motif consisting of a set of atoms. Repeating the motif through a translation a leads to a kind of linear crystal. If this linear crystal is submitted to a translation by a vector b (not collinear with a), then by 2b, 3b, etc., a plane crystal is obtained. To obtain the global crystal, the plane crystal is then thought to be submitted to a translation by a vector c not coplanar with plane (a, b), then by 2c, 3c, etc. 3. Motif is the French word for pattern. It is adopted in crystallographic English, with the present meaning.

6

Symmetry and Physical Properties of Crystals

1.4. Basic assumptions of geometrical crystallography In order to describe crystal structures, we make three assumptions: 1.

The crystal is assumed to be inﬁnite. This assumption is reasonable, since the order of magnitude of the lengths a, b and c of the period vectors is a few angströms (1 Å = 10−1 nm). A small crystal with dimensions of the order of a micrometer, for example, contains linear sequences several thousands of periods long.

2.

The thermal vibrations of atoms about a perfectly deﬁned average position is neglected. Our description assumes that the atoms are ﬁxed at these average positions.

3.

The crystal is assumed to be perfectly triply periodic, i.e. not to feature any defect. Crystal defects can then be described with respect to the perfect crystal. The study of crystal defects is a broad subject, outside the scope of this book. A brief introduction to one type of defect, the dislocation line, is given in Complement 13C.

1.5. Anisotropy of physical properties The beautiful crystal faces that can be observed in natural minerals and in some synthetic crystals are related to the very strong anisotropy of the growth rates as a function of growth direction. Figure 1.7 explains how the only faces that remain after some growth has occurred are those perpendicular to the directions where the growth rate is much smaller than in other directions. We consider, at time t = 0, three face orientations denoted as 1, 2 and 3, with one of them (noted 2) growing at a velocity v2 twice larger than the two others (faces 1 and 3). We see that at time t all faces are present, whereas, at time 2t, face 2 has disappeared.

v2t

v1t 1

2 v1t

2 3

t=0

t

2t

Figure 1.7: Growth at diﬀerent rates of crystal faces. Face 2, with growth velocity v 2 twice larger than that, v 1 , of faces 1 and 3, ends up disappearing.

Chapter 1 – Introduction

7

The habit, i.e. the very regular special shape, of crystals thus shows that the growth velocity is much smaller along certain directions, ﬁnite in number, than in all other directions. This is one of the expressions of the anisotropy of the physical properties of crystals. In this case, anisotropy is discontinuous while, for most other physical properties, it is continuous, meaning that the value of a physical quantity such as the expansion of a material along a given direction, under the inﬂuence of a rise in temperature, varies continuously as direction is varied. This anisotropy of their physical properties is a characteristic of crystals. Describing it involves the use of tensors. This will be the topic of the second part of this book, starting with Chapter 9.

1.6. Remarks on the scope of this book : topics left out The aim of this book is to describe the structure and properties of perfectly ordered crystalline solids. We have seen that we therefore leave aside glasses or amorphous solids, the structure of which is close to that of a liquid set at a given instant [1]. Neither shall we mention liquid crystals or mesophases [2]. They often consist of rod-shaped molecules, which assemble parallel to one another, forming plane layers. In a given layer, the molecules may be ordered only at short range, as in a liquid, but the existence of these parallel layers denotes partial order, whence the term crystal. Neither will we deal with quasi-crystals, discovered in 1984 [3] (see also [4]). They can be obtained through ultra-fast quenching of metallic alloys (e.g. Al–Mn–Si or Al–Fe–Cu). They do not feature the triple periodicity of crystals. They do however, like crystals, feature orientation symmetry: all properties observed along a given direction are reproduced along the directions deduced from the former through the action of the symmetry elements in the point group of the quasi-crystal. Because there is no translation symmetry, these point groups are diﬀerent from those that are consistent with the crystalline state.

8

Symmetry and Physical Properties of Crystals

Complement 1C. Crystal growth This complement is no more than a glimpse into the fascinating art and science of crystal growth. The variety of techniques and of characterization methods it encompasses is exempliﬁed by a recent handbook of crystal growth (see Further reading): it comprises over 1800 pages, with a short table of contents spanning 14 pages and a detailed table of contents of 30 pages.

1C.1. Natural growth of single crystals The largest producer of single crystals is nature. Large (centimeter-range) single crystals of many naturally occurring compounds, usually called minerals, have long been valued for their beauty and have raised many questions that led to understanding the structure of matter. Their characteristic habits, with well-developed natural faces, occur when their growth process involves isotropic enough an environment as well as enough space. The typical process, hydrothermal growth, is based on the slow deposition of a solute as the temperature of the solution changes, and it is often associated with high pressures. Among the most popular examples of minerals are quartz SiO2 (rock crystal), calcite CaCO3 (Iceland spar), diamond C, pyrite FeS2 (fool’s gold, Fig. 1.3a). They may well, through their beauty, have kindled the reader’s interest for crystals and symmetry. Other materials crystallize very easily, at room pressure and room temperature, from solutions: this is the case for sodium chloride NaCl (rocksalt), or copper sulfate CuSO4 . Crystallization is then a convenient way of purifying the material.

1C.2. Crystal growth for scientiﬁc purposes Growing single crystals is an important support activity for basic research. A meaningful investigation of anisotropic macroscopic properties, for example magnetism, electrical or heat conduction, or the ferroelectricity (see Sect. 15.2) of materials, requires single crystals, where the directional properties are the same throughout the sample. The growth must then be followed by the precise determination of the orientation of the crystal, so that a sample with well-deﬁned crystal directions can be cut out. The laboratory techniques cover a broad range of approaches, depending on the chemical properties, melting temperature, etc. of the material. Thus soluble materials can often be made to crystallize in a controlled way by slow evaporation of the solvent, while refractory materials will have to be molten in an induction furnace, often in the form of a levitating drop without contact with a crucible to avoid contamination, and cooled in a temperature gradient. The Bridgman method provides for cooling of a larger molten sample, in contact with a small crystal used as a seed, in a temperature gradient. Another broadly used technique is the Czochralski method, where the seed is dipped into the melt and slowly pulled out at the same time that it is rotated. In the ﬂux-growth method, the material to be crystallized is molten together with another material which is

Chapter 1 – Introduction

9

not incorporated in the solid but lowers the melting temperature; with proper setting of the temperature evolution over days or weeks, good crystals can be obtained. From another point of view, single crystals are necessary for many structure determinations using X-ray or neutron diﬀraction techniques. However, detailed examination of the validity of the usual data processing procedures (“kinematical approximation”, if necessary with corrections) indicates that the crystals should not be big. Typical optimal sizes are tenths of a millimeter for X-rays, and a few millimeters for neutrons. Furthermore, nearly perfect crystals are not desirable for this kind of study, so that the requirements are, happily, close to what crystal synthesis produces. The preparation of single crystals of biological material, such as proteins, in their native hydrated form, is a crucial step toward the determination of their structure. The approach usually consists in trying many recipes at the same time, using boxes with tens of compartments which are ﬁlled with drops of the material with various values of the pH or other possibly relevant parameters. The growth of crystals of biomaterials was investigated in microgravity conditions in satellites, in order to eliminate the inﬂuence of convection. A similar quest is the motivation for crystal growth in gels.

1C.3. Industrial crystal growth It may appear paradoxical to ﬁnd that almost perfect crystals, the production of which is almost invariably fraught with diﬃculties, are required by industry rather than by basic research. Semiconductor device production is based on the preparation of many chips per single-crystal silicon substrate. They are cut from huge single crystal ingots, typically 300 mm in diameter in 2009 and a meter long, without any linear defect (dislocation line, see Complement 13C). This achievement in crystal growth technology was the result of large eﬀorts toward a thorough understanding of crystal defects. These eﬀorts were undertaken because it was vital to keep at a very low level the number of defective chips grown on a wafer. One side-eﬀect of the mastery achieved in the preparation and processing of silicon crystals was that elaborately shaped parts like inkjet printer nozzles were made out of silicon single crystals. Crystals with intermediate sizes are grown industrially for applications in optoelectronics (for example lithium niobate LiNbO3 – see Sect. 19.2). Other materials routinely produced in the form of excellent crystals, but comparable neither in quantities nor in quality with silicon, are SiO2 (quartz) and AlPO4 (berlinite) for piezoelectric oscillators (see Chap. 15), and SiC (silicon carbide) for electronic devices. Industrial single crystals of diamond are available in a wide range of crystal quality and crystal size, with use as diﬀerent as oil drill rigs and optical elements (monochromators) for synchrotron radiation X-rays. Synthetic diamond does not reach into the jewelry range yet, but other gemstones (emerald, sapphire. . . ) are routinely produced artiﬁcially as substitutes for their natural

10

Symmetry and Physical Properties of Crystals

counterparts. Again in a very diﬀerent area, turbine blades for jet planes are made of single crystals of an aluminum-base alloy in view of their mechanical strength at the high temperatures involved.

1C.4. Growth of single-crystal thin ﬁlms Films with very small thickness, down to the nanometre range, are important for nanotechnology and basic science, e.g. for the investigation of semiconductor quantum well or quantum dot devices, or of magnetic recording and readout heads for hard disk drives. Their manufacture involves a range of approaches, based on vapor-phase or liquid-phase epitaxy (the growth of single crystal ﬁlms on single-crystal substrates, with a close relation between their orientations), or molecular-beam epitaxy (MBE). The latter is a highly sophisticated technique involving extreme vacuum and requiring stringent purity controls. Multilayers, consisting of several stacked thin ﬁlms exhibiting structural coherence at the interfaces, are industrially manufactured by sputtering techniques. They make up the tunnel magnetoresistance (TMR) read heads4 used in 2011 in the hard disk drive of all recent computers. Mastering epitaxic growth processes implies a very good knowledge of the surfaces on which the layers are to be grown. This makes the study of surface crystallography very important. The description of crystal surfaces is dealt with in Section 3.8 of this book.

Further reading I.V. Markov, Crystal Growth for Beginners (World Scientiﬁc, Singapore, 1996) G. Dhanaraj, K. Byrappa, V. Prasad, M. Dudley, Springer Handbook of Crystal Growth (Springer, 2010)

4. Wikipedia, Tunnel magnetoresistance, http://en.wikipedia.org/wiki/Tunnel magnetoresistance (as of Nov. 7, 2013)

Chapter 1 – Introduction

11

References [1] S.R. Elliot, Physics of Amorphous Materials, 2nd edn. (Longman Scientiﬁc and Technical, Harlow, Essex, 1990) [2] P.G. de Gennes and J. Prost, The Physics of Liquid Crystals (Oxford University Press, Oxford, 1993) [3] D. Shechtman, I. Blech, D. Gratias, J.W. Cahn, Metallic phase with longrange orientational order and no translational symmetry, Phys. Rev. Lett. 53, 1951–1953 (1984) [4] C. Janot and J.M. Dubois, Les quasicristaux, matière à paradoxes (EDP Sciences, Les Ulis, 1998)

Chapter 2

Symmetry operations The aim of this chapter is to detail the notions of symmetry operations and symmetry elements, which are basic in the description of crystals. The ﬁnal section introduces some notions related to symmetry groups.

2.1. Isometries An isometry is a geometrical transformation which transforms an object either into an identical object (this is called a direct or proper isometry) or into its image with respect to a mirror plane (it is then called an indirect or improper isometry). A direct, or orientation preserving, isometry conserves the handedness (right or left) of a trihedron, whereas an indirect, or orientation reversing, isometry reverses it. Successively applying two isometries, i.e. applying the composition or “product” of these isometries obviously is an isometry. The product of two direct isometries is a direct isometry since the transform is at each stage identical to the object. The product of a direct and an indirect isometry is an indirect isometry, and the product of two indirect isometries is a direct one. More generally, the product of any number of isometries is indirect if it involves an odd number of indirect isometries, and a direct isometry otherwise. The isometries are: a rotation around a given axis, a translation (both of these are direct isometries), symmetry with respect to a point, also called inversion with respect to this point, symmetry with respect to a plane (both being indirect isometries), and all operations resulting from the composition (or product) of two or several of these isometries. It is convenient to deﬁne a special indirect isometry which is very much used in crystallography: rotoinversion (or rotation-inversion), the product of a rotation around an axis and of an inversion with respect to a point located on this axis. Two special rotoinversions should be mentioned here: rotoinversion by 2π, which is nothing else than inversion, and rotoinversion with angle π, which is

© Springer Science+Business Media Dordrecht 2014 C. Malgrange et al., Symmetry and Physical Properties of Crystals, DOI 10.1007/978-94-017-8993-6_2

13

14

Symmetry and Physical Properties of Crystals

equivalent to symmetry with respect to the plane perpendicular to the axis used for the rotation, and going through the point O used for the inversion (Fig. 2.1). z’ m

M

O

H

P M’ z

Figure 2.1: Rotoinversion by π around axis zz , the point used as a center of symmetry being O. M is the transform of M through this rotoinversion because m is the transform of M through a rotation by π around axis zz and M is the transform of m through the symmetry with center O. M is symmetric of M with respect to plane P, perpendicular to zz and going through O. We thus see that the set of isometries can also be deﬁned as the set of the rotations, rotoinversions, translations and their combinations, since inversion and symmetry with respect to a plane are two special rotoinversions.

2.2. Symmetry operations. Symmetry elements For some objects, an isometry (or several isometries) transform(s) the object into an object that is not only identical but superimposable on the object itself, and which is therefore undistinguishable from the latter. These isometries which leave the object invariant are the symmetry operations for this object.

2.2.1. n-fold rotations and axes Consider as an example the two-handled jug shown on Figure 2.2a. A rotation by 180◦ around axis zz changes the jug into a jug that superimposes upon itself: the rotation by 180◦ around zz is a symmetry operation for this object. The product of this symmetry operation with itself is a rotation by 360◦ around zz , or the identity operation since, following this symmetry operation, the object is superimposed upon itself point for point. Axis zz is said to be a 2-fold axis for the jug, or alternatively the jug is said to have a 2-fold axis as a symmetry element. The regular square-based pyramid shown on Figure 2.2b has a 4-fold axis because the rotation by 2π/4 = π/2 around zz is a symmetry operation for this pyramid. The existence of a 4-fold axis implies that the object has 4 symmetry

Chapter 2 – Symmetry operations

15

operations, viz. the rotation by π/2 around the axis, which can for example be noted as R, its product with itself R2 , which is the rotation by π, the product of R2 by R, i.e. R3 , which is the rotation by 3π/2, and operation R4 , equal to the rotation by 2π or identity operation, noted E. In a general way, if an object has an n-fold rotation axis, it has n symmetry elements which are the rotations by 2π/n, 2(2π/n), . . . , k(2π/n) . . . and ﬁnally the rotation by n(2π/n) = 2π which is the identity operation. The cylinder of revolution shown on Figure 2.2c has an inﬁnite-order axis, because a rotation by any angle, however small, is a symmetry operation. z

z

z

z’

z’

z’

(a)

(b)

(c)

P

Figure 2.2: Objects featuring symmetry elements We will see (Sect. 3.3.2) that crystals, because of their triple periodicity, can only have 2-, 3-, 4- or 6-fold axes.

2.2.2. n-fold rotoinversions and n-fold rotoinversion axes, denoted as n ¯ -fold axes If a rotoinversion by angle 2π/n (the product of a rotation by 2π/n around a given axis and an inversion with center O located on this axis) is a symmetry operation for an object, the latter is said to have an n ¯ -fold rotoinversion axis. We have seen that the rotoinversion by 2π is identical with inversion. The existence of a ¯1 axis is therefore equivalent to the existence of a center of symmetry. The existence of a ¯2-fold axis (for which the associated symmetry operation is the rotoinversion by π) is equivalent to the existence of a symmetry plane (or mirror) perpendicular to the axis and going through the center used for inversion (see Fig. 2.1). It should be noted, in contrast, that the axis deﬁning the rotation is not a 2-fold axis for the object, just as the inversion center that is used in this rotoinversion is not a center of symmetry for the object. A rotoinversion is the product of a rotation and an inversion. It is therefore quite distinct from the rotation itself and the inversion itself.

16

Symmetry and Physical Properties of Crystals

We will see that crystals can only have as rotoinversion axes ¯1, ¯2, ¯3, ¯4 or ¯6 axes. An example of an object having a ¯4-axis is shown on Figure 2.3a. It is a sphenohedron, a solid having four vertices A, B, C and D with the following properties: segments AB and CD have equal lengths and are perpendicular to each other. They are perpendicular to the axis zz which intersects them in their middles, H and K respectively (Fig. 2.3b and 2.3c). The rotoinversion by π/2 around zz , with point O, the middle of HK, as the inversion center, transforms point A into C, point B into D, C into B and D into A. It thus transforms the sphenohedron into itself. Axis zz is therefore a ¯4 axis for this solid. In contrast, it is quite clear that the sphenohedron has neither a 4-fold axis nor an inversion center. z’ A B

A

H B

D A O

O, H, K B C D

C

D

K

C z

(a)

(b)

(c)

Figure 2.3: (a) A perspective view of a sphenohedron. (b) The sphenohedron ABCD. Axis zz is a ¯4-fold axis for this object. (c) Projection of points A, B, C and D on a plane perpendicular to zz .

2.2.3. Translations If a translation by a vector t is a symmetry operation for an object, the product of n translations t, equal to the translation nt, is also a symmetry operation. Since n can be arbitrarily large, the object is necessarily inﬁnite, in contrast to the above cases of rotations and rotoinversions. Such an object is said to be periodic with period t. For example, Figures 2.4a and 2.4b, obtained from a simple pattern which is outlined by a thin dotted line (something like a music note for 2.4a and a set of two such notes for 2.4b), repeated to inﬁnity by translation t, have translation t (and all the translations nt) as symmetry operations. Figure 2.4b furthermore has a symmetry plane or mirror, perpendicular to the plane of the ﬁgure and going through the line uu . If the inﬁnite sequence of patterns of Figure 2.4a is submitted to a translation by a vector t (not collinear with t) and its multiples, the obtained ﬁgure (Fig. 2.5) has the translations nt + n t (n and n integers) as symmetry operations.

Chapter 2 – Symmetry operations

17

t

(a)

u

t

u’

(b)

v

t

v’

(c)

Figure 2.4: Figures which are periodic with period vector t (assuming they extend to inﬁnity). The motif or pattern is marked with a thin dotted line on each ﬁgure.

t’ t

Figure 2.5: A plane ﬁgure with periodicity along two directions

2.2.4. Screw axes and glide mirrors In Sections 2.2.1 and 2.2.2, we deﬁned two types of symmetry elements : axes of order n and axes of order n ¯ . In crystallography, further symmetry elements must be deﬁned. They are associated to the symmetry operations which are the products (also called compositions) of rotations or rotoinversions and translations. These elements are on the one hand screw axes, the associated symmetry operations of which are the products of a rotation and a translation parallel to the rotation axis and, on the other hand, glide mirrors, the associated symmetry operations of which are the products of an operation of symmetry with respect to a plane (a mirror operation) and a translation parallel to this plane. Consider two examples: an object with a screw axis and an object with a glide

18

Symmetry and Physical Properties of Crystals

mirror. Since the associated symmetry operations include a translation part, these objects are necessarily inﬁnite. Screw axis: consider a helical staircase, in which all steps have the same height, and such that when walking up by one step we rotate around the central axis by an angle equal to a submultiple of 2π, for example 30◦ . The operation product of a rotation by 30◦ around the axis of the staircase and a vertical translation equal to the height of the steps is a symmetry operation for this staircase, under the proviso, of course, that we imagine it to have inﬁnite height. This staircase has a screw axis coinciding with its axis. Glide mirror: Figure 2.4c is formed from a motif (the pattern of Fig. 2.4b altered by translating one of the two notes by t/2), repeated to inﬁnity by translation t. This periodic ﬁgure thus features translation t and its multiples as symmetry operations. It also features a less obvious symmetry operation: the product of the symmetry with respect to a plane perpendicular to the plane of the ﬁgure and going through line vv and the translation by vector t/2. The corresponding symmetry element is called a glide mirror, the glide being the translation t/2.

2.2.5. Note We have deﬁned the following symmetry elements: n-fold axes, for which the associated symmetry operations are a rotation by 2π/n and its multiples, n ¯ -fold axes, for which the associated symmetry operations are a rotoinversion by 2π/n and its multiples, mirrors for which the associated symmetry operation is symmetry with respect to the plane of the mirror, screw axes for which the associated symmetry operations are the product of a rotation and a translation and its multiples, and glide mirrors, for which the associated symmetry operations are the product of a symmetry with respect to the plane of the mirror and a translation and its multiples. We see that the term “symmetry element” covers two notions: on the one hand a geometrical object, a line or a plane, and on the other hand the set of symmetry operations which are associated to it.

2.3. Introduction to symmetry groups In this introduction, we restrict discussion to ﬁnite objects. This rules out symmetry operations that include a translation. The symmetry operations which a ﬁnite object can feature are thus the rotations and rotoinversions, the latter including symmetry with respect to a point and symmetry with respect to a plane (Sect. 2.1 and Fig. 2.1). We show that the symmetry operations of a ﬁnite object form a group. Let us ﬁrst recall the deﬁnition of a group.

Chapter 2 – Symmetry operations

19

A group is a set of elements among which one can deﬁne an internal composition law that is associative and includes a neutral element e such that, for any element a of the group, ae = ea = a. Each element of the group must have an inverse a−1 such that aa−1 = a−1 a = e. For the symmetry operations featured by an object, the internal composition law is the product of two symmetry operations, i.e. the succession of these two operations. The neutral element is the identity operation, and the inverse operations of the elementary operations, such as rotation by an angle ϕ around an axis, symmetry with respect to a point O or symmetry with respect to a plane P are thus evident: they are respectively the rotation by an angle −ϕ around the same axis, symmetry with respect to the same point O, and symmetry with respect to the same plane P. The symmetry operations of an object thus form a group. Let us take as an example the symmetry operations of the jug of Figure 2.2a. We saw that the axis zz is a 2-fold axis to which are associated the two following symmetry operations: rotation by an angle π around zz , which we will denote as A, and the operation A2 or rotation by 2π around zz , which is the identity operation, noted as E. Furthermore, this jug has two other symmetry elements. The plane P going through zz and parallel to the two handles is a symmetry plane or mirror. Let m1 be the operation “symmetry with respect to plane P”. It is clear that m21 = E. In the same way, the plane P going through zz and perpendicular to plane P is a symmetry element. If m2 is the operation “symmetry with respect to plane P ”, then m22 = E. We have thus deﬁned four symmetry operations, viz. A, m1 , m2 and E. We can easily draw the multiplication table for these operations (Tab. 2.1). Table 2.1: Multiplication table for the group of symmetry operations of the jug of Figure 2.2a E

A

m1

m2

E

E

A

m1

m2

A

A

E

m2

m1

m1

m1

m2

E

A

m2

m2

m1

A

E

The product of A and m1 is noted m1 A, the rule being that the order of operations is read from right to left, so that operation A is here followed by operation m1 . This product m1 A is shown at the intersection of line m1 and row A. It is easily checked that this product m1 A is equal to m2 . Consider any point M. The plane perpendicular to the 2-fold axis going through M is

20

Symmetry and Physical Properties of Crystals

represented on Figure 2.6 where uu and vv are the traces, on this plane, of mirrors P and P respectively. v’ (P’ m2) M”

M O

u

u’ (P m1)

M’ v

Figure 2.6: Showing the product of operation A (rotation by π around axis zz perpendicular to the plane of the ﬁgure) and operation m1 (symmetry with respect to the plane P, with trace uu on the ﬁgure). The transform of M through A is M , the transform of M through m1 is M . M is obtained from M through symmetry with respect to plane P , i.e. through operation m2 . We notice that, on each row and each column of the table itself (surrounded by a bold line on Tab. 2.1), all the elements of the group appear, and each appears only once. This is a general result which is derived in Appendix 4A. The generating elements of a group are the elements which are suﬃcient to deﬁne the group. The set of elements of the group is obtained by multiplying these elements with one another or with their inverses. In the example chosen, we see that A and m1 are generating elements of the group, but alternative choices of generating elements are A and m2 or m1 and m2 . A group is said to be commutative if, for any two elements a and b of the group, ab = ba. We see that the group considered above is commutative since the multiplication table is symmetric with respect to its diagonal.

2.4. Exercises Exercise 2.1 We want to derive the following result: if an object has an n-fold axis and a mirror that goes through this axis, it has n mirrors which go through the axis and which enclose between one another angles π/n. 1.

Consider two mirrors, M1 and M2 , enclosing between them an angle α. We note zz the intersection of the two mirrors. Let m1 and m2 be the symmetry operations with respect to plane M1 and to plane M2 respectively. Use a geometrical argument to show that the product m2 m1 is equal to a rotation by 2α around zz , so that m2 m1 = Rotzz (2α).

2.

Deduce from this result that m1 = m2 Rotzz (2α) and m2 = Rotzz (2α)m1 .

Chapter 2 – Symmetry operations

21

3.

Use the result of (2) to obtain the result we seek, viz. that, if an object has an n-fold axis and a mirror that goes through this axis, it has n mirrors deduced from the ﬁrst one through rotations by π/n and its multiples around the axis.

4.

Enumerate the eight symmetry operations of the square-based regular pyramid of Figure 2.2b.

5.

Write down the multiplication table of the group consisting of these symmetry operations. Is it commutative?

Exercise 2.2 Determine the symmetry elements of the two molecules shown below: Br Br

H C

C H

C2 H2 Br2

H H

H C

C

C H

C3 H4

C2 H2 Br2 : the two H atoms and the carbon to which they are linked are coplanar. Their plane is perpendicular to the plane containing the other C atom and the two Br atoms which are linked to it. C3 H4 : the three C atoms are aligned and equidistant. The plane containing the C atom at one end of the chain and the two H atoms which are linked to it is perpendicular to the plane containing the C atom at the other end of the chain and the two H atoms which are linked to it. The angle between the C–H bonds is identical in the two planes. Exercise 2.3 Show that the proper symmetry elements of a cube are: three 4-fold axes, four 3-fold axes and six 2-fold axes.

Chapter 3

Crystal lattices This chapter deﬁnes the crystal lattice, which directly expresses the triple periodicity of the crystal, and all the derived notions: reciprocal lattice, crystal systems and Bravais lattices. The ﬁnal part of the chapter shows how this deﬁnition of the crystal lattice is extended for the study of the surface of crystals.

3.1. Direct lattice We saw that crystals are characterized by their periodicity in three directions. They are deﬁned by a crystal motif consisting of a well-deﬁned set of atoms, which repeats through periodic translations in three non-coplanar directions. We will see that a lattice is associated to this triple periodicity, and that the crystal can thus be deﬁned by its motif and its lattice, which is called direct (in contrast with the so-called reciprocal lattice which will be deduced from the direct lattice in Sect. 3.2).

3.1.1. Unit cell, row Two-dimensional lattice We start with examples of two-dimensional periodic systems because they are easier to represent and to understand, and are well suited for introducing many notions. Figure 3.1a is an example. It shows an elementary motif, a general triangle, periodically reproduced in two diﬀerent directions with period vectors respectively a and b, forming an inﬁnite object. This inﬁnite object features translation symmetry, meaning that any translation t = ua + vb, where u and v are two integers, transforms the object into an object undistinguishable from itself. If we replace the triangle by a group of atoms, we obtain a twodimensional crystal. Now suppose we replace the elementary motif by a point located near the motif in some position, general (i.e. with no special requirement) but perfectly deﬁned with respect to the motif (Fig. 3.1b). We obtain a regular lattice of points which deduce from one another through the set of translations ua + vb

© Springer Science+Business Media Dordrecht 2014 C. Malgrange et al., Symmetry and Physical Properties of Crystals, DOI 10.1007/978-94-017-8993-6_3

23

24

Symmetry and Physical Properties of Crystals

(u and v being integers). This set of points (Fig. 3.1c) is called the crystal lattice, and each point is a lattice node. We can thus deﬁne a plane crystal lattice, with basis vectors a and b, as a set of points M, called nodes, deﬁned by the relation OM = ua + vb where O is any point, chosen as the origin node, and u and v are integers.

b

b

a

a

(b)

(a) M b”

b

a”

a O b’

a’

d

c

(c)

Figure 3.1: (a) A two-dimensional periodic ﬁgure; (b) the associated crystal lattice; (c) examples of primitive cells (a, b), (a , b ), (a , b ) and a multiple unit cell (c, d) Any line going through two nodes is called a row. The parallelogram built on a and b is called the primitive cell for this lattice, and the vectors a and b are its basis vectors. We note that the whole crystal lattice is obtained by paving the whole plane with parallelograms identical to this one, and placing one node at each of the vertices. Each node then belongs to four cells, and counts for 1/4 per cell. One cell then contains 4 times (1/4 node), i.e. one node per cell, and this is why such cells are called primitive cells. It is sometimes designated as a simple unit cell. Vectors a and b are not the only ones which can deﬁne a simple unit cell for a given lattice. Other possible choices are for example the vector pairs a and b , or a and b (Fig. 3.1c). In contrast, vectors c and d deﬁne a cell which also contains a node at its center. The cell is no more a primitive cell, it is termed a multiple cell. Alternative denominations are nonprimitive or centered (or centred) cell. The whole crystal lattice is obtained by setting next to one another such cells, which have a node in common at each of

Chapter 3 – Crystal lattices

25

their vertices and a node at their center. The cell spanning c and d is a double unit cell because it contains two nodes: the node at the center which belongs to only one cell, and the four vertex nodes, each belonging to four cells and counting for 1/4, thus in total another node.1 The number of nodes associated to one unit cell is called the multiplicity or order of the unit cell: thus the cell (c, d) has multiplicity 2. The area of a primitive cell deﬁned by vectors a and b is equal to the norm of the cross product a × b. The areas of all the other primitive cells (such as those deﬁned by a and b or a and b for instance) are identical, each of them being equal to the area associated to one node. The area of a unit cell of order n is equal to n times the area of a primitive cell, since it is equal to the area associated to n nodes. The multiplicity of the cell deﬁned by the vectors f = ua + vb and g = u a + v b (u, v, u , v being integers) can also be determined by computing the cross product f × g: (ua + vb) × (u a + v b) = (uv − u v) (a × b) the norm of which is equal to (uv − u v) a × b, thus an integer (possibly equal to 1) times the area of the primitive cell since u, v, u , v are integers. The crystal lattice is characterized by choosing, if possible, a primitive cell which directly reﬂects the symmetry of the crystal lattice. Suppose for example that the lattice consists of nodes at the vertices of rectangles positioned next to one another (Fig. 3.2a). The lattice is then deﬁned by a rectangular primitive cell, (a, b), and not by a general parallelogram. Now suppose the primitive cell (a, b) of the lattice is a lozenge (Fig. 3.2b). The lattice features symmetry elements: mirrors perpendicular to the plane of the ﬁgure and parallel to the diagonals of the lozenges. These symmetry elements show up immediately if the choice is made of a unit cell with basis vectors c and d, orthogonal to each other, with a node in its center. The lattice is thus deﬁned by a double rectangular cell termed centered rectangular. Three-dimensional lattice The above notions are easily generalized to the case of three-dimensional crystals. The crystal motif is then reproduced through non-coplanar translations a, b, c, and their multiples. Replacing the motif by a point located in some arbitrary but perfectly deﬁned position with respect to the motif produces a regular lattice of points, deduced from one another by translations ua+vb+wc with u, v, w integers. The crystal lattice is then deﬁned by choosing for the origin a point O and drawing all the points M that are the ends of vectors OM = ua + vb + wc with u, v, w integers. The set of points M deﬁnes the crystal lattice and each of these points is called a lattice node. Point O is the origin node.

1. Another way of counting the nodes per unit cell is to imagine the cells to be slightly displaced, so that the lattice nodes no more coincide with the vertices. The nodes in each unit cell are then distinctly visible.

26

Symmetry and Physical Properties of Crystals

b a

d c

b a

(b)

(a)

Figure 3.2: Rectangular plane lattices. The parallelograms built on a and b are primitive cells in both ﬁgures. However, in Figure (a), this parallelogram, actually a rectangle, describes the full symmetry of the lattice. In contrast, describing the symmetry in Figure (b) requires a multiple (centered) unit cell. Any line going through two nodes M and M is called a row, and it contains an inﬁnity of nodes (Fig. 3.3). The vector MM joining nodes M and M has the form u a + v b + w c, where u , v and w are integers since OM and OM are of this form. There is an inﬁnity of rows parallel to MM . The one that goes through the node at origin O goes through node N such that ON = MM = u a + v b + w c. Let u, v and w be integers proportional to u , v and w and mutually prime. The vector ON = ua + vb + wc is the smallest lattice vector parallel to this direction. It deﬁnes the period of the nodes on this row, and more generally on the family of rows parallel to this one, which will be denoted as [uvw].

N’

M’

N

M

O

Figure 3.3: An example of a crystal row. The plane of the ﬁgure is deﬁned by the nodes M and M and the node O taken as the origin.

Chapter 3 – Crystal lattices

27

The parallelepiped spanning the three basis vectors a, b and c is the primitive cell of the crystal (Fig. 3.4a). The sign of the vectors a, b and c is conventionally chosen so that the trihedron a, b, c be direct. The volume of the cell is equal to the mixed product (a, b, c), equal to a · (b × c). We will see that the requirement for a unit cell to feature all the symmetry elements of the crystal lattice leads to deﬁning multiple cells, just as in the case of two-dimensional lattices. Multiple cells can be base-centered if two opposite faces are centered, face-centered if all the faces are centered (Fig. 3.4b), or body-centered if there is a node at the center of the cell. This is why multiple cells are also called centered cells. The multiplicity (or order) of the unit cell is obtained by counting the number of nodes per unit cell, taking into account that a node at the center of the cell adds one node per cell, while a node at the center of a face, belonging to two distinct cells, counts for 1/2.

c1

c

c b b1

b

a a1

a

(a)

(b)

Figure 3.4: (a) Primitive cell of a crystal lattice; (b) multiple, facecentered unit cell with basis vectors a1 , b1 , c1 , and the corresponding primitive cell with basis vectors a, b, c The multiplicity of a cell spanning the crystal lattice vectors a1 , b1 , and c1 such that a1 = u1 a + v1 b + w1 c, b1 = u2 a + v2 b + w2 c, c1 = u3 a + v3 b + w3 c, (ui , vi , wi being integers) can be determined from the volume of the unit cell, equal to the mixed product (a1 , b1 , c1 ). This can be written in matrix from: ⎛

⎞ ⎛ ⎞ a1 a ⎝ b1 ⎠ = U ⎝ b ⎠ c1 c

28 with

Symmetry and Physical Properties of Crystals

⎞ u1 v1 w1 U = ⎝ u2 v2 w2 ⎠ u3 v3 w3 ⎛

Hence (a1 , b1 , c1 ) = det U (a, b, c) where (a, b, c) is the volume of the primitive cell. The multiplicity is thus given by det U .

3.1.2. Lattice planes Any plane that goes through three non-aligned nodes is called a lattice plane. It contains an inﬁnity of nodes, which form a two-dimensional lattice. The set of lattice planes parallel to a given lattice plane describes the whole crystal lattice. In other words, the lattice can be described as the set of the lattice planes of a given family. This can be done in an inﬁnity of ways, since any family of lattice planes can be chosen as the starting point. This is shown on Figure 3.5, based, for simplicity, on a lattice with a primitive cubic cell. The basis vectors a, b and c are therefore mutually orthogonal and have the same length a. The ﬁgure represents the projections of the nodes of this lattice onto a plane perpendicular to one of the basis vectors, for example c. The projected nodes form a square lattice of points, and we have represented the traces of a few families of lattice planes perpendicular to the plane of the ﬁgure. Note, and this is valid whatever the crystal lattice, that the planes of a given family are equally spaced (equidistant) and that the node density in the planes is smaller the closer the planes are to one another.2 Now consider a general crystal lattice, with a primitive cell deﬁned by vectors a, b and c (forming a direct trihedron, as mentioned before). We choose an origin node O and axes Ox, Oy and Oz respectively parallel to a, b and c. We focus on the lattice plane parallel to vector c and containing two nodes M and N belonging to plane (a, b) (Fig. 3.6). The other lattice planes belonging to the same family intersect plane (a, b) along equidistant lines shown dotted on the ﬁgure. One of them goes through the origin O; we label it with number 0. The successive equidistant neighboring planes are numbered 1, 2, 3, . . . , on the side towards which the vectors a and b point, and those located in the other half-space are numbered successively −1, −2, −3, etc. One of these planes necessarily goes through node A, the end of vector a; let h be the integer that characterizes it. In the case shown in the ﬁgure, h = 3, so that it is the third plane. Plane number 1, the one closest to origin, intersects axis Ox at a point with coordinate a/h (a/3 on Fig. 3.6). In the same way, there is necessarily a plane of the same family, numbered k (2 on the ﬁgure), that goes through 2. This is easily veriﬁed by noting that the number n of nodes per unit volume has a given value for a given crystal lattice. On the other hand, on a lattice plane belonging to a given family, the number of nodes per unit area ρ is such that ρ = nd where d is the distance between two successive lattice planes of this family.

Chapter 3 – Crystal lattices

29

node B, the end of vector b. Plane 1 intersects axis Oy at b/k (b/2 on the ﬁgure). Since we chose a family of planes parallel to the basis vector c, plane 1 intersects axis Oz at inﬁnity.

b a

a

Figure 3.5: Projection of a simple cubic lattice on a plane perpendicular to the basis vector c. Various families of lattice planes perpendicular to the plane of the ﬁgure project along the dotted lines. k

y

M B b A O a

x N

−1 0 1 2 3 4

h

Figure 3.6: Traces on plane (a, b) of a family of lattice planes parallel to basis vector c

30

Symmetry and Physical Properties of Crystals

Now let us apply the same reasoning to a general family of lattice planes (Fig. 3.7). The reasoning is based on the fact that a family of lattice planes contains all the lattice nodes, and that all the planes of this family are equidistant. One of these planes, noted P0 , goes through the origin O of the lattice. Another one, called P, goes through the node located at A such that OA = a. There are, between these planes, a number n of equidistant intermediate planes, which divide segment a into an integral number of segments, each with length a/n. Let us call P1 the one which is closest to P0 . y x

z

A

P B a P’ P1 P0

C c Q

b N

M O

P−1

Figure 3.7: A family of lattice planes. P0 is the plane belonging to the family that goes through the origin O of the crystal lattice. P1 and P-1 are the two planes of this family that are closest to O. This plane P1 intersects segment OA at a point M with coordinates (a/h, 0, 0) where h is a positive or negative integer depending on whether plane P1 intersects axis Ox on the side of the positive or negative x, and n = |h|. Similarly, since one of the planes of the family necessarily goes through node B such that OB = b, plane P1 intersects axis Oy at a point N with coordinates (0, b/k, 0) where k is an integer. Finally a plane of the family goes through node C, such that OC = c, and plane P1 intersects axis Oz at Q, with coordinates (0, 0, c/l) where l is an integer. The numbers h, k, l are integers which can be positive or negative. The equation of this plane P1 in the coordinate system Oxyz has the form αx + βy + γz = δ. Writing that the coordinates of M, N and Q satisfy this equation, we obtain: b c a = δ, β = δ, γ = δ. h k l Replacing α, β and γ by their values as a function of δ, the equation of plane P1 becomes x y z h + k + l = 1. a b c α

Chapter 3 – Crystal lattices

31

Let us select as the length unit on each of the axes the length of the corresponding basis vector, viz. a on Ox, b on Oy and c on Oz, and this is the choice we will use throughout this book, this equation becomes hx + ky + lz = 1.

(3.1)

The equation of the n-th plane of this family, on the same side as P1 with respect to the origin, is hx + ky + lz = n while the n-th plane on the other side is hx + ky + lz = −n. The equation of the plane belonging to this family and going through the origin is hx + ky + lz = 0. (3.2) The integers h, k and l are mutually prime. Let us show this by supposing they were not. Then we could write h = mh , k = mk and l = ml where m, h , k and l are integers. Equation (3.1) would then become 1 . m It must be satisﬁed by all the nodes of the plane, the coordinates of which are integers. h , k and l being integers, this is impossible if m = 1 since then 1/m would not be an integer. h x + k y + l z =

This family of lattice planes is designated as (hkl) and we will remember that: The notation (hkl), where h, k and l are mutually prime integers, designates a family of lattice planes such that the plane of the family closest to the node at origin intersects axis Ox at a/h, axis Oy at b/k and axis Oz at c/l. h, k and l are called the Miller indices of this family of lattice planes. Note that the integers h, k and l are placed between parentheses while the integers deﬁning a family of rows (Sect. 3.1.1) are noted between square brackets. Note: the planes parallel to a have the designation (0kl) since they intersect axis Ox at inﬁnity. Similarly the planes parallel to b have the form (h0l) and those parallel to c the form (hk0). Application: what condition must h, k, l and u, v, w satisfy for a plane (hkl) and a row [uvw] to be parallel to each other? Row [uvw] is by deﬁnition parallel to the vector OM = ua + vb + wc. The plane parallel to the row and going through origin therefore contains the point M, with coordinates u, v, w and, from (3.2), we must have hu + kv + lw = 0. We note that: A row [uvw] is parallel to a plane (hkl) if and only if hu + kv + lw = 0.

32

Symmetry and Physical Properties of Crystals

3.1.3. Wigner-Seitz cell Solid-state physicists often use another way of subdividing direct space into identical cells containing one lattice node per cell. The center of these cells is chosen on one lattice node. The mediating planes of the segments joining the chosen node to the ﬁrst nodes on the various rows which point out of this node are then drawn. The smallest volume thus created around the node is the Wigner-Seitz cell (Fig. 3.8). This cell is primitive because it is associated to a single lattice node, but it is not a parallelepiped. In Section 3.2, we will deﬁne another lattice of points, deduced from the direct lattice, which is called the reciprocal lattice. The same construction applied to this reciprocal lattice deﬁnes a cell called the ﬁrst Brillouin zone.

Figure 3.8: Wigner-Seitz cell of a plane lattice. The segment in dotted lines connects the origin to a node which does not take part in the construction of the cell because the mediator of this segment is outside the cell.

3.2. Reciprocal lattice 3.2.1. Introduction based on diﬀraction The above considered lattice is deﬁned in the space of the crystal, and this is why it is called the direct lattice. Another associated lattice is very much used: it is called the reciprocal lattice and plays a part in the phenomena of diﬀraction by crystals and more generally in all problems of wave propagation in crystals. It is the space of wave vectors, the dimensions of which are reciprocal lengths. It should be mentioned that the crystallographers’ tradition is to write a plane wave w, with amplitude a and frequency ν (angular frequency ω = 2πν) in the form w = a cos 2π(k · r − νt), so that the norm of the wave-vector is equal to 1/λ where λ is the spatial period of the wave, i.e. the wavelength. This is in contrast with the tradition of optics and of most physicists, who write w = a cos(k · r − ωt), so that the norm of their k is equal to 2π/λ. This is summarized in Table 3.1 below. The triple periodicity in the position of atoms in a crystal leads to a plane wave of monochromatic X-rays incident on the crystal being diﬀracted into well-deﬁned directions.

Chapter 3 – Crystal lattices

33

Table 3.1: Deﬁnition of the wave-vector k as used in various areas of physics Crystallography

w = a cos 2π(k · r − νt) ||k|| = 1/λ

Optics, quantum mechanics, solid state physics

w = a cos(k · r − ωt) ||k|| = 2π/λ

Consider a crystal whose primitive cell is deﬁned by the vectors a, b and c. This crystal consists in a motif and its transforms by all the translations of the crystal lattice τ = ua + vb + wc (u, v, w integers). Let ko be the wave-vector of the incident wave. This wave interacts with the electrons in the atoms of the crystal motif. Assume for simplicity that the motif consists of a single atom. This monoatomic motif scatters into all space a spherical wave with the same wavelength. For an observer located far enough from the crystal, this spherical wave can be considered as plane with a wave-vector kd . The waves scattered by two identical motifs located at P and Q, a vector τ = ua + vb + wc apart, have a path diﬀerence δ = PK − HQ such that: δ = (sd − so ) · τ where sd and so are unit vectors along kd and ko respectively. sd K

so

P ko

H

kd Q

Figure 3.9: Scattering of a plane wave by two crystal motifs separated by a vector τ All the plane waves scattered by all the motifs are in phase if δ = nλ (n an integer) for all τ , so that (sd − so ) · τ = nλ or

(kd − ko ) · τ = n

(3.3)

since |kd | = |ko | = 1/λ. This is seen to involve calculating the dot product of a vector τ of direct space, expressed in a non-orthonormal basis {a, b, c}, and a vector of the space of wave-vectors. This dot product is easily written if the vector kd − ko is expressed in a basis {a∗ , b∗ , c∗ } such that the dot product of a∗ and a is equal to 1 while the dot products of a∗ and b or c are zero, with similar

34

Symmetry and Physical Properties of Crystals

relations for b∗ an c∗ : a∗ · a = 1

a∗ · b = 0

a∗ · c = 0

∗

b∗ · b = 1

b∗ · c = 0

∗

c∗

b · a=0 c · a=0

· b=0

(3.4)

∗

c · c=1

Let u∗ , v ∗ and w∗ be the components of the vector kd − ko in the basis {a∗ , b∗ , c∗ }. The vector kd − ko is expressed as kd − ko = u∗ a∗ + v ∗ b∗ + w∗ c∗ . Taking into account Equations (3.4), condition (3.3), with n an integer, takes the form u∗ u + v ∗ v + w ∗ w = n which must be veriﬁed for all integral values of u, v and w. This requires that u∗ , v ∗ and w∗ be integers. The reciprocal lattice of a crystal is deﬁned as the set of points N obtained starting from an origin O and such that ON = ha∗ + kb∗ + lc∗ where h, k and l are integers. The points N are the nodes of the reciprocal lattice and O the origin node. We just showed that the diﬀraction condition is equivalent to the condition that the components u∗ , v ∗ and w∗ , in the basis of the reciprocal lattice, of the scattering vector (or diﬀraction vector) kd − ko be integers, i.e. that this scattering vector be a vector joining two nodes of the reciprocal lattice. The diﬀraction condition is thus very simply expressed thanks to the reciprocal lattice. Furthermore, we see on Equations (3.4) that: The reciprocal lattice of the reciprocal lattice is the direct lattice. This results from the fact that the ﬁrst column of Equations (3.4) deﬁnes a as a function of a∗ , b∗ and c∗ just like the ﬁrst row deﬁnes a∗ as a function of a, b and c, etc.

3.2.2. Alternative deﬁnition of the reciprocal lattice The relations (3.4) show that a∗ is perpendicular to b and c, hence parallel to the cross product b × c. We can thus write: a∗ = α (b × c). Furthermore, since a · a∗ = 1, we have: a · a∗ = α a · (b × c) = αv0 = 1, with v0 = (a, b, c) the volume of the crystal unit cell. Hence α = 1/v0 and therefore a∗ = (b × c)/v0 .

Chapter 3 – Crystal lattices

35

In the same way, we obtain b∗ = (c × a)/v0 , and

c∗ = (a × b)/v0 .

(3.5)

Relations (3.5) directly deﬁne the reciprocal lattice with respect to the basis vectors of the direct lattice. This is the most usual deﬁnition of the basis vectors of the reciprocal lattice. Further, since the direct lattice is the reciprocal lattice of the reciprocal lattice, a = (b∗ × c∗ )/v0∗ , b = (c∗ × a∗ )/v0∗ , c=

(a∗

×b

∗

(3.6)

)/v0∗ ,

with v0∗ the volume of the reciprocal unit cell, i.e. the volume of the parallelogram built on a∗ , b∗ and c∗ .

3.2.3. Properties of the reciprocal lattice Basic property Consider the lattice plane P1 of the family (hkl) that is closest to the origin O of the direct lattice. A point M of this plane has coordinates x, y, z in basis {a, b, c}: OM = xa + yb + zc. From relation (3.1), x, y and z then satisfy the relation hx + ky + lz = 1

(3.7)

where we recall that the integers h, k and l are mutually prime. Consider the vector h∗ of the reciprocal lattice with components h, k and l h∗ = ha∗ + kb∗ + lc∗ . The properties of the reciprocal lattice encountered above show that OM · h∗ = hx + ky + lz and, taking into account (3.7), OM · h∗ = 1. Let H be the projection of M on the vector h∗ (Fig. 3.10), with norm ||h∗ || . OM · h∗ = OH ||h∗ || = 1 and

OH = 1/|| h∗ || = constant.

36

Symmetry and Physical Properties of Crystals

H M

P1 dhkl h* O P0

Figure 3.10: Two neighboring (hkl ) planes: P0 goes through the origin of the lattice and P1 is its ﬁrst neighbor. We deduce that all points of plane P1 project onto vector h∗ at the same point H, which means that plane P1 is perpendicular to the vector h∗ . On the other hand, OH is the distance of plane P1 to the plane of the family (hkl) which goes through O. This is the distance dhkl between two successive planes in the family (hkl). We thus obtain dhkl =

1 . ||h∗ ||

(3.8)

Basic property: The planes (hkl) are perpendicular to the row [hkl]∗ of the reciprocal lattice and their distance dhkl is equal to the reciprocal of the modulus of the vector h∗ = ha∗ + kb∗ + lc∗ . It is important to recall that the vector h∗ which is being discussed as a way of calculating the distance between two neighboring lattice planes of family (hkl) connects the origin of the reciprocal lattice3 to the ﬁrst reciprocal lattice node on the row [hkl]∗ that goes through the origin, since h, k, l are mutually prime. X-ray diﬀraction can also be described in terms of selective mirror reﬂection of X-rays on the lattice planes. The condition for constructive interference is given by Bragg’s law 2dhkl sin θ = nλ where λ is the wavelength, θ the complement of the angle of incidence on the lattice planes, and n the order of the reﬂection. Bragg’s law can also be written 2(dhkl /n) sin θ = λ and the reﬂection of order n on the lattice planes (hkl) described by arbitrarily introducing reﬂecting planes parallel to the lattice planes (hkl), and n times closer to one another, their distance being dhkl /n. This distance dhkl /n between reﬂecting planes is equal to 1/(n||h∗ ||), i.e. the reciprocal of the norm of a new vector h∗ = nh∗ of 3. For simplicity, we select the origin of the reciprocal lattice as coinciding with that of the direct lattice.

Chapter 3 – Crystal lattices

37

the reciprocal lattice connecting the origin of the reciprocal lattice to the n-th node on the row [hkl]∗ . One then speaks of a reﬂection nh, nk, nl such that 2dnh,nk,nl sin θ = λ with dnh,nk,nl = 1/||h∗ || where h∗ is now the reciprocal lattice vector connecting the origin to the n-th node along row [hkl]∗ . In this way each reciprocal lattice node is associated to a reﬂection, the ﬁrst node in each row corresponding to the reﬂection of order 1 and the n-th node to the reﬂection of order n. We note that everything concerning the reciprocal lattice is indicated by a star: the basis vectors a∗ , b∗ , c∗ , a row [hkl]∗ and a family of lattice planes (hkl)∗ . Since the lattice reciprocal to the reciprocal lattice is the direct lattice, we can similarly state that: The planes (hkl)∗ of the reciprocal lattice are perpendicular to the row [hkl] of the direct lattice. Volume of the reciprocal unit cell Let us substitute, in the expression (3.5) for a∗ , the vector c by its expression (3.6) as a function of the reciprocal lattice vectors. We obtain a∗ = (b × (a∗ × b∗ ))/v0 v0∗ . Using the expression of the double cross product A × (B × C) = B (A · C) − C (A · B), and relations (3.4), we obtain a∗ = [a∗ (b · b∗ ) − b∗ (b · a∗ )]/v0 v0∗ = a∗ /v0 v0∗ . This shows that

v0 v0∗ = 1.

(3.9)

Note: all of the above discussion refers to unit cells associated with a single lattice node (primitive cells). The reciprocal lattice of a multiple unit cell must be deﬁned using a primitive cell. It is however possible to then describe the reciprocal lattice using a multiple reciprocal unit cell (see Sect. 3.7.3).

3.2.4. Crystallographic calculations Calculation of lattice distances The lattice distance dhkl in a family of lattice planes (hkl) is determined by relation (3.8), which yields: 1 = (ha∗ + kb∗ + lc∗ )2 , d2hkl where the basis vectors a∗ , b∗ and c∗ of the reciprocal lattice are determined as a function of the basis vectors a, b and c of the direct lattice through relations (3.5).

38

Symmetry and Physical Properties of Crystals

We thus obtain 1 = (ha∗ + kb∗ + lc∗ )2 d2hkl = h2 a∗2 + k 2 b∗2 + l2 c∗2 + 2hk a∗ · b∗ + 2kl b∗ · c∗ + 2lh c∗ · a∗ . (3.10) In Section 3.4.2, we will deﬁne the crystal systems, and derive the expressions for the values of dhkl in each of them. Search for the indices of a lattice plane parallel to two rows of the direct lattice We are looking for the plane (hkl) which is parallel to rows [u1 v1 w1 ] and [u2 v2 w2 ]. First method: We saw, at the end of Section 3.1.2, that the condition for row [uvw] of the direct lattice to be parallel to plane (hkl) is that hu + kv + lw = 0.

(3.11)

We apply this condition to both rows: hu1 + kv1 + lw1 = 0, hu2 + kv2 + lw2 = 0. We deduce that k l h = = . v1 w2 − w1 v2 w1 u2 − u1 w2 u1 v2 − v1 u2

(3.12)

Second method: Let n1 = u1 a + v1 b + w1 c and n2 = u2 a + v2 b + w2 c be vectors parallel to the two rows respectively. The plane we are looking for, being parallel to both vectors, is perpendicular to the cross product of the vectors n1 and n2 , which is expressed as n1 × n2 = (u1 a + v1 b + w1 c ) × (u2 a + v2 b + w2 c) = (v1 w2 − w1 v2 )(b × c) + (w1 u2 − u1 w2 )(c × a) + (u1 v2 − v1 u2 )(a × b).

(3.13)

Taking into account Equations (3.5) which deﬁne the basis vectors of the reciprocal lattice, we obtain: n1 × n2 = v0 [(v1 w2 − w1 v2 )a∗ + (w1 u2 − u1 w2 )b∗ + (u1 v2 − v1 u2 )c∗ ].

(3.14)

Chapter 3 – Crystal lattices

39

We see that The cross product of two vectors of direct space lattice is parallel to a vector of the reciprocal lattice, a result which will be used in the next paragraph. Let us write the cross product (3.14) in the following form: n1 × n2 = v0 [h a∗ + k b∗ + l c∗ ] where h = v1 w2 − w1 v2 , k = w1 u2 − u1 w2 and l = u1 v2 − v1 u2 are integers since ui , vi and wi are integers. If h , k , l are not mutually prime, call h, k, and l the mutually prime integers proportional to them (h = nh, k = nk, l = nl). Thus n1 × n2 is parallel to the vector [hkl]∗ of the reciprocal lattice, with h, k and l mutually prime. Such a vector is perpendicular to the plane (hkl) of the direct lattice, which is the plane we are looking for. We thus retrieve relations (3.12). Search for the row [uvw] parallel to the intersection of planes (h1 k1 l1 ) and (h2 k2 l2 ) First method: We apply condition (3.11) to the row [uvw] and to the planes (h1 k1 l1 ) and (h2 k2 l2 ). h1 u + k1 v + l1 w = 0, h2 u + k2 v + l2 w = 0. We deduce that v w u = = . k1 l2 − l1 k2 l1 h2 − h1 l2 h1 k2 − k1 h2

(3.15)

Second method: The vectors V∗1 = h1 a∗ + k1 b∗ + l1 c∗ and V∗2 = h2 a∗ + k2 b∗ + l2 c∗ are perpendicular to the planes (h1 k1 l1 ) and (h2 k2 l2 ) respectively. The row we are looking for is therefore perpendicular to these vectors, hence parallel to the cross product V∗1 × V∗2 . The latter is parallel to a vector of the space reciprocal to reciprocal space, i.e. a vector of direct space. Following the same approach as in (3.13) and (3.14), we obtain: V∗1 × V∗2 = v0∗ [(k1 l2 − l1 k2 ) a + (l1 h2 − h1 l2 ) b + (h1 k2 − k1 h2 ) c] and we retrieve the result (3.15).

40

Symmetry and Physical Properties of Crystals

3.3. Properties of crystal lattices 3.3.1. Centers of symmetry All nodes of a crystal lattice are centers of symmetry for the lattice, as we can easily see, for example on the two-dimensional lattice of Figure 3.1c. The same applies to the centers of the unit cells. Therefore All crystal lattices feature centers of symmetry.

3.3.2. n-fold and n ¯ -fold axes consistent with the crystalline state We will now show that: A crystal lattice can only feature n-fold axes of order 2, 3, 4 or 6. The same applies to n ¯ -fold axes, which can only be 1¯ , 2¯ , 3¯ , 4¯ or 6¯ axes. First derivation: Consider a vector V of the crystal lattice. If the lattice features a symmetry element, one of the symmetry operations S associated to this element will transform V into a vector V = SV which is also a lattice vector. V and V , being lattice vectors, have integral components with respect to the coordinate system deﬁned by the basis vectors a, b and c of the crystal unit cell. The coeﬃcients in the matrix representing operation S in this basis are therefore integers, and its trace is also an integer. If a lattice features an n-fold axis, let us call S the rotation by α = 2π/n around this axis, denoted An . The trace of the matrix representing an operator does not depend on the basis chosen (orthonormal or not) to represent this operator. We choose to represent this operator in an orthonormal frame such that Oz coincides with axis An hence through matrix S ⎛ ⎞ cos α − sin α 0 S = ⎝ sin α cos α 0 ⎠ . 0 0 1 The trace of S is equal to 1 + 2 cos α: therefore 2 cos α must be an integer. Furthermore, |2 cos α| ≤ 2 and the only possible values of 2 cos α are therefore: −2, −1, 0, 1, 2. If cos α = ±1, α = 0 or π. There is a 1-fold axis, i.e. no symmetry (if α = 0), or a 2-fold axis (if α = π). If cos α = ±1/2, α = ±2π/3 or ±π/3, and there is a 3-fold axis or a 6-fold axis. If cos α = 0, α = ±π/2 and there is a 4-fold axis. The only possible values for n are therefore n = 1 (trivial), 2, 3, 4 and 6.

Chapter 3 – Crystal lattices

41

The derivation is the same for the n ¯ axes. Operation S is then the rotation by α = 2π/n followed by an inversion with respect to a center located on the rotation axis. The matrix representing this operation is then −ES where S is the above matrix and E is the unit matrix. The trace of this matrix is −(1 + 2 cos α), which must be an integer; therefore 2 cos α is an integer with modulus less or equal to 2. We thus retrieve the preceding results, hence the same consequences, viz. the possible existence of ¯1, ¯2, ¯3, ¯4 and ¯6 axes. A ¯1 axis is identical to a symmetry center, already mentioned in Section 3.3.1. Second (geometrical) derivation This derivation applies more conveniently to rotation axes. We use the result, independently derived in Section 3.3.4 below, that an n-fold axis is perpendicular to a family of lattice planes, hence to a set of lattice vectors. Let V = AB be an elementary vector of the crystal lattice (i.e. a vector connecting two neighboring nodes), perpendicular to the n-fold axis. Let us perform onto AB the symmetry operation S, a rotation by α = 2π/n around the n-fold axis that goes through node A (Fig. 3.11). The vector AB becomes AB , which therefore is a lattice vector. Operation S, performed n − 1 times, is a symmetry operation. It is a rotation by (n − 1)α = 2π − α = −α (modulo 2π). We recall that two angles are equal modulo 2π if their diﬀerence is an integer times 2π. Let us apply this rotation −α to vector AB using the axis located at B:4 BA becomes BA , a lattice vector. It is easy to show that vector B A is parallel to AB. Its length is equal to AB(1 − 2 cos α) and it is a lattice vector. It is therefore equal to an integer times AB. Thus (1 − 2 cos α) is an integer and 2 cos α is an integer. We retrieve the same results as above. A’

B’

A

– B

Figure 3.11: A and B are two neighboring nodes on a crystal lattice featuring n -fold axes perpendicular to the plane of the ﬁgure.

3.3.3. The direct lattice and the reciprocal lattice have the same symmetry elements Let S be a symmetry operation (rotation or rotoinversion) featured by a given direct crystal lattice. It therefore transforms the direct lattice R into a lattice R with which it is superimposed, so that SR = R ≡ R.

4. Translation symmetry implies the existence of an n-fold axis at B if there is one at A.

42

Symmetry and Physical Properties of Crystals

Let a , b and c be the transforms of a, b and c under S. We can write a = S a,

b = S b and c = S c.

The reciprocal lattice R∗ of R can be obtained from a , b and c or from a, b and c since R and R are identical. We want to show that the symmetry operation S transforms R∗ into itself. Let us deﬁne R∗ through a∗ , b∗ and c∗ such that: a∗ = (b × c )/v0 = (Sb × Sc)/v0 = ±S(b × c)/v0 = ±Sa∗ = S(±a∗ ). Similarly, b∗ = S(±b∗ ) and c∗ = S(±c∗ ). The sign + or − depends on the nature (proper or improper) of S but R∗ can be deﬁned using −a∗ , −b∗ and −c∗ just as well as using a∗ , b∗ and c∗ . We therefore see clearly that the lattice R∗ is transformed by S into itself. S is thus a symmetry operation for the reciprocal lattice.

3.3.4. Geometrical relation between the symmetry axes and the crystal lattice We now show that: Any symmetry axis (rotation or rotoinversion axis) is parallel to a row of the direct lattice and perpendicular to a lattice plane. Let S be the elementary symmetry operation associated to the n-fold axis (rotation by 2π/n) or n ¯ −fold axis (rotation by 2π/n followed by an inversion). It transforms a vector V parallel to the axis into an equal (rotation case) or opposite (rotoinversion case) vector. SV = ±V

or

(S ∓ E)V = 0

where E is the unit operator. In the basis a, b, c, the coeﬃcients of the matrix S representing operation S are integers since S transforms a lattice vector into another lattice vector. The same applies to S ± E. Solving the equation system (S ± E)V = 0, we ﬁnd that the components u, v and w of vector V are such that u/w = p/r and v/w = q/r with p, q and r integers, whence u/p = v/q = w/r. Since p, q and r are integers, the symmetry axis is parallel to a row5 [p q r] of the lattice. The same derivation can be applied to the reciprocal lattice, which also features this symmetry element (Sect. 3.3.3). The symmetry axis is thus also parallel to a reciprocal lattice row, and thus perpendicular to a lattice plane of the direct lattice (see Sect. 3.2.3). 5. The integers p, q and r are not necessarily mutually prime. If they are not, they should be replaced by numbers proportional to p, q and r and mutually prime, in order to deﬁne the row adequately.

Chapter 3 – Crystal lattices

43

3.3.5. The lattice is at least as symmetrical as the crystal Pierre and Jacques Curie stated in 1894 a very far-reaching principle which is now called the Curie principle. It will be introduced in Chapter 9 (Sect. 9.5.2) and widely used in the second part of this book. One of the direct consequences of this principle can be stated as follows: the physical properties of a crystal are at least as symmetrical as the crystal. The crystal lattice describes one property of the crystal, viz. its triple periodicity. Therefore the crystal lattice must be at least as symmetric as the crystal. This property will be derived in Section 4.2.3 and used in Section 5.6 to determine the crystal lattice of a crystal as a function of the symmetry properties of the crystal itself.

3.4. Crystal systems The results mentioned in this section are not derived but the enumeration of crystal systems introduced below is so natural that it can be performed before their precise deﬁnition is introduced (Sect. 5.6 and Chap. 6). Suﬃce it to say that a crystal system is characterized by the smallest unit cell, primitive or multiple (centered), which features all the symmetry elements of the corresponding lattice.

3.4.1. Two-dimensional crystal systems Let us recall that the symmetry elements of a plane object are perpendicular to the plane of the object, and that a center of symmetry O is then equivalent to a 2-fold axis perpendicular to the plane and going through O. There are four plane crystal systems, shown in Table 3.2. Table 3.2: The plane crystal systems System Unit cell shape

Oblique

Rectangular

Square

Hexagonal

parallelogram

rectangle

square

lozenge with angle 120° 120°

Bravais lattices

p

p c (centered)

p

p

They are: the oblique (general primitive cell), rectangular (rectangular primitive cell), square (square primitive cell), and hexagonal (primitive cell in the shape of a lozenge with angle 120◦ ) systems. We note that a lozenge-shaped primitive cell produces a rectangular centered lattice. The rectangular centered double cell evidences more explicitly the symmetry elements of the lattice,

44

Symmetry and Physical Properties of Crystals

viz. the mirror symmetry planes parallel to the basis vectors of the centered rectangular cell. We will see (Sect. 3.7) that they are the primitive (p) and centered (c) Bravais lattices.

3.4.2. Three-dimensional crystal systems There are seven three-dimensional crystal systems, deﬁned and illustrated in Table 3.3. The basis vectors of the unit cell are always called a, b, c and the trihedron a, b, c is chosen as direct. The angles in the cell faces are denoted as α = (b, c), β = (c, a) and γ = (a, b). The seven systems are the following: Triclinic: the unit cell is a general parallelepiped, deﬁned by its three angles α, β, and γ (in Greek, klinos means angle) and the lengths a, b and c of the three basis vectors. Monoclinic: the unit cell is a right prism with bases in the shape of a parallelogram, deﬁned by just one angle (whence the name) since the two others are right angles, and the lengths a, b and c of the three basis vectors. The basis vector perpendicular to the two others was long selected as the vector b, and the angle to be deﬁned is then β. Nowadays a frequent choice, more consistent with the choices for the other systems, is to take it as vector c, and the angle to be deﬁned is then angle γ. Orthorhombic (from the Greek orthos = right): the unit cell is a rectangle parallelepiped. All that is to be deﬁned are the three lattice parameters a, b and c. Tetragonal: the unit cell is a right prism with square base (a rectangle parallelepiped in which two opposite faces are square). One chooses to call a and b the basis vectors forming the square and c the basis vector which is perpendicular to them. Two lattice parameters must therefore be deﬁned: a = b and c. Rhombohedral (or trigonal): the unit cell is a rhombohedron, i.e. a parallelepiped in which all the faces are equal (Fig. 3.14a). The only values to be deﬁned are the lattice parameter a = b = c and the angle α = β = γ. We can visualize a rhombohedron as a cube which has been drawn out or compressed along one of its major diagonals. In a cube, the major diagonals are 3-fold axes. If a cube is drawn out or ﬂattened along one of its major diagonals while retaining the equality of the edges, this diagonal remains a 3-fold axis while the others are no longer 3-fold axes. The rhombohedral lattice is described in more detail in Section 3.6.2. Hexagonal: the unit cell is a special right prism. Its base is a lozenge with one angle equal to 120◦ . The basis vector perpendicular to the two others is c. Two cell parameters must be deﬁned: a = b and c. Cubic: the unit cell is a cube, and the only parameter to be deﬁned is a = b = c.

Chapter 3 – Crystal lattices

45

Table 3.3: The seven three-dimensional crystal systems Crystal system Shape of unit cell

Parameters

Polyhedron

Bravais lattices

Triclinic

a b c

general parallelepiped

P

c b

c

Monoclinic

a a b c general

b

a a b c general

b a c

Orthorhombic

cb

P, A (or B) right prism with parallelogram-shaped base P, C (or A)

a b c

right prism with rectangular base

P A (or B or C) I, F

a b c

right prism with square base

P, I

a b c

rhombohedron

R (P)

a b c 120°

right prism with 120° lozenge base

P

a b c

cube

P, I, F

a

Tetragonal

c

b a

Rhombohedral (Trigonal) ab

c

Hexagonal b

Cubic

c a

cb a

46

Symmetry and Physical Properties of Crystals

In each crystal system, the lattice distance dhkl can be calculated as a function of the basis vectors a∗ , b∗ and c∗ of the reciprocal lattice using formula (3.10). For all systems except for the triclinic and rhombohedral systems, this formula can be simpliﬁed, and dhkl is easily expressed as a function of the parameters of the direct lattice, i.e. of the lengths a, b and c of the basis vectors and the angles α, β and γ between these vectors. Some of these calculations are the topics of exercises, and the result for the various crystal systems is given in Table 3.4. For the triclinic and rhombohedral lattices, it is convenient to use a quantity called the metric tensor, which is introduced in Appendix 3A. The metric tensor is widely used in numerical calculations for crystallography. Table 3.4: Lattice distances for the various crystal systems dhkl

Crystal system

Triclinic Monoclinic

Orthorhombic

1 − cos2 α − cos2 β − cos2 γ + 2 cos α cos β cos γ A 2 2 h2 hl sinβ / + cl 2 + kb sin2 β − 2 ac cos β a2 if b // 2-fold axis of the cell l 2 2 h2 k2 sinγ / sin γ − 2 hk ab cos γ a2 + b2 + c if c // 2-fold axis of the cell 2 1 / ha2 +

k2 b2

+

l2 c2

Rhombohedral

2 a / h2 + k 2 + l2 ac 1+2 cos3 α−3 cos2 α a 2 2 2 2

Hexagonal

2 a / 43 (h2 + k 2 + hk) + l2 ac

Cubic

√ a / h2 + k 2 + l2

Tetragonal

(h +k +l ) sin α+2(hk+kl+lh)(cos2 α−cos α)

h2 k2 l2 hk 2 2 sin α + sin β + sin2 γ + 2 (cos α cos β − cos γ) 2 2 2 a b c ab kl hl + 2 (cos α cos γ − cos β) + 2 (cos β cos γ − cos α) ac bc

A=

Chapter 3 – Crystal lattices

47

3.5. Examples of reciprocal lattices 3.5.1. Monoclinic lattice The unit cell is deﬁned by the lengths a, b, c of the basis vectors and by the angle β between vectors a and c (if the choice is to denote as b the basis vector parallel to the 2-fold axis of the cell). The volume v0 of the unit cell is equal to abc sin β. b×c v0 c ×a b∗ = v0 a×b ∗ c = v0 a∗ =

and and and

1 ; a sin β 1 b∗ = ; b 1 ∗ c = . c sin β

a∗ =

Vector b∗ is parallel to vector b. The vectors a∗ and c∗ are in the plane of vectors a and c and perpendicular to c and a respectively. The angle between a∗ and c∗ is equal to π − β (Fig. 3.12). The hexagonal lattice can be treated the same way (Exercise 3.4). a

a*

9

b,b*

c* c

Figure 3.12: Basis vectors of a monoclinic lattice and of the corresponding reciprocal lattice projected on a plane perpendicular to vector b (parallel to the 2-fold axis). The vectors b and b∗ are perpendicular to the plane of the ﬁgure and point upwards.

3.5.2. Orthorhombic, tetragonal and cubic lattices In these three lattices, the basis vectors a, b and c are mutually orthogonal: therefore the vectors a∗ , b∗ and c∗ are parallel to vectors a, b and c respectively, and their lengths a∗ , b∗ and c∗ are equal to 1/a, 1/b and 1/c respectively. In the tetragonal lattice, a = b and a∗ = b∗ . In the cubic lattice where a = b = c, the three basis vectors of the reciprocal lattice have the same length a∗ = b∗ = c∗ = 1/a.

48

Symmetry and Physical Properties of Crystals

3.6. Hexagonal lattice and rhombohedral lattice 3.6.1. Hexagonal lattice The hexagonal lattice is deﬁned from two basis vectors a and b with the same length, enclosing an angle of 120◦ (Fig. 3.13), and a vector c perpendicular to a and b. In the basal plane deﬁned by the vectors a and b, we could just as well select the vector couples b and d (or d and a) where d is the vector deduced from b through a rotation by 120◦ around the 6-fold axis of the lattice (parallel to c). These three vectors a, b and d are related by: a + b + d = 0.

b d

a

Figure 3.13: Hexagonal lattice; projection of the nodes onto a plane perpendicular to c To evidence, in the lattice plane notation, the 3-fold symmetry of these vectors, a fourth index i is added between indices k and l, leading to the notation (hkil) such that the lattice plane closest to origin intersects the vectors a, b, d and c at a/h, b/k, d/i and c/l. It can be shown (Exercise 3.5) that the relation h+k+i=0

or

i = −(h + k)

applies. This four-index notation makes it possible to easily determine the lattice planes equivalent through the symmetry operations of the crystal (Exercises 3.5 and 5.6). The notation (hkil) is sometimes replaced by (hk.l) to show that one deals with a hexagonal lattice. This four-index notation cannot apply to rows [uvw], since it is then meaningless.

3.6.2. Rhombohedral lattice Consider a rhombohedral lattice. The unit cell is a rhombohedron shown on Figure 3.14a. Its basis vectors are LP = a, LM = b and LN = c. The plane MNP is a (111) plane, noted as Π1 on Figure 3.14b. We note as Π0 the (111) plane containing node L, Π2 the one containing nodes Q, R and S and Π3 the one containing T.

Chapter 3 – Crystal lattices

49 T

T 3 R

R

S

Q

N c

P a

M

2

S

N 1

R’

Q

L

M L’

P

M

S’#

B& P

(a)

& #

N

b 0

&

#

& #Q’

A

#

J

L

(b)

(c)

Figure 3.14: Rhombohedral lattice: (a) primitive cell; (b) showing the succession of (111) planes; (c) projection of the lattice onto plane Π1 , perpendicular to the 3-fold axis (empty circles for the nodes of Π0 and Π3 , full circles for the nodes of Π1 , and crosses for the nodes of Π2 ) The nodes in each of these (111) planes form a hexagonal plane lattice since they are at the vertices of adjacent equilateral triangles. The nodes of planes Π0 (containing L) and Π3 (containing T) project onto Π1 at L , the center of triangle MNP, and on all equivalent points (empty circles in Fig. 3.14c), i.e. at the centers of every other of the equilateral triangles formed by the hexagonal plane lattice of Π1 . The nodes of plane Π2 such as Q, R and S project at the centers of the other triangles (crosses, and for example Q , R and S , the projections of Q, R and S respectively). We immediately see on Figure 3.14c that the rhombohedral lattice can be described by a triple hexagonal unit cell, with basis vectors A = PJ = NM = NL + LM = b − c, B = PN = PL + LN = c − a, C = LT = LN + NR + RT = a + b + c, so that ﬁnally

A = b − c, B = c − a, C = a + b + c.

This unit cell is triple because it contains the nodes Q and T which project onto Π1 at Q and L respectively. We can add to the basis vectors A and B a vector D deﬁned as in Section 3.6.1, i.e. such that A+B+D=0 so that D = MP = a – b.

50

Symmetry and Physical Properties of Crystals

It is current practice to describe a rhombohedral lattice in this way, through its triple hexagonal unit cell, with basis vectors A, B and C, because it is much easier to handle. Conversely, the basis vectors of the rhombohedral unit cell are obtained from those of the hexagonal unit cell through the relations C D−B + , 3 3 C A−D b= + , 3 3 C B−A c= + . 3 3 a=

3.7. Bravais lattices 3.7.1. Why they are needed We are not going to systematically enumerate the Bravais lattices. This will be done in Chapter 6. Here we introduce them after showing why it is of interest to deﬁne them. In many cases, the primitive cell considered as an individual object has symmetry lower than the symmetry of the lattice, while a multiple (or centered) cell can evidence the symmetry of the lattice. A ﬁrst example is the case of a rhombohedral unit cell with angle equal to 60◦ . When the whole lattice is represented, we ﬁnd that the nodes are at the vertices of cubes and at the centers of the faces of these cubes (Fig. 3.15a). The derivation is simpler when starting from the face-centered cubic (fcc) lattice. It is then easy to see that the parallelepiped in which the basis vectors A, B, C connect a vertex P to the centers Q, R, S of the faces starting in P is a rhombohedron with apical angle 60◦ , since the triangles PQR, PRS and PSQ are equilateral. Thus the primitive cell, taken individually, does not feature all the symmetry elements of the face-centered cubic lattice (in particular the 4-fold axes). This is the reason for choosing the quadruple face-centered cubic cell. Thus, for three-dimensional lattices, several multiple cells are used to describe lattices featuring more symmetry elements than the primitive cell shows. Each multiple cell deﬁnes a lattice mode. If the cell that describes the lattice is a primitive cell, the lattice mode is said to be primitive, and it is noted as P. If the cell is base-centered (double cell), the lattice mode is A or B or C depending on whether the centered bases are respectively the faces (b, c) or (c, a) or (a, b). The generic designation for this type of centering is S (for side-face centered). If the cell is body-centered (double cell), the lattice mode is I (as in “inside”), and if the cell has all of its faces centered (quadruple cell), it is noted F (as in “face”). The reader will easily check that these multiple cells do deﬁne a crystal lattice. In contrast, a cell to which one would attempt to add

Chapter 3 – Crystal lattices

51

2c* P’ R’ c

P

A* B*

S

A b

Q B C

Q’

S’

2b*

2a*

R

C*

a

(b)

(a)

Figure 3.15: Face-centered cubic lattice (a) and its reciprocal lattice (b) nodes at the centers of four pair-wise parallel faces does not deﬁne a crystal lattice (Exercise 3.6). To each crystal system there correspond one or several lattice modes. The set of all these lattice modes form the 14 Bravais lattices, distributed over the 7 crystal systems. The rule for determining which Bravais lattice, hence which unit cell, should describe a given structure is to choose the cell (a) featuring the symmetry of the lattice and (b) with the smallest volume. Two examples are very illuminating: the face-centered cubic lattice quoted above, and the body-centered cubic lattice, for which the primitive cell is a rhombohedron with angle α = 109.47◦ (cos α = − 1/3) (Fig. 3.16).

A

B

C

Figure 3.16: The body-centered cubic lattice. The primitive cell is deﬁned by the vectors A, B and C.

52

Symmetry and Physical Properties of Crystals

One may ask why all of the lattice modes are not deﬁned in each of the crystal systems. Actually, some multiple (centered) cells provide no improvement over the primitive cell or over some other multiple cell with lower multiplicity, or again the multiple cell does not feature the symmetry of the lattice any more. Consider for example the tetragonal lattice. There is no advantage in deﬁning a tetragonal lattice in which the square base (a, b) is centered, since the unit cell built on the half-diagonals of the square, a and b , and the vector c is tetragonal too (Fig. 3.17). Furthermore, it can be shown that a face-centered tetragonal unit cell can be described by a centered cell twice as small (Exercise 3.10). A tetragonal unit cell with two opposite non-square faces centered is not a tetragonal cell, since the lattice built on this cell does not have a 4-fold axis any more. The only multiple tetragonal unit cell is the tetragonal body-centered cell, for which no primitive cell can represent the tetragonal symmetry of the lattice.

c

b’

b

a’

a

Figure 3.17: A tetragonal lattice with its square base centered does not need to be considered. The primitive cell, with basis vectors a , b and c, is tetragonal.

3.7.2. The fourteen Bravais lattices The last column of Table 3.3 indicates for each crystal system the various lattice modes. There are all together 14 Bravais lattices (1 triclinic, 2 monoclinic, 4 orthorhombic, 2 tetragonal, 1 rhombohedral, 1 hexagonal, and 3 cubic). Two rows were set aside for the monoclinic system, in order to be able to state the denomination of the base-centered lattices. In this case, the bases which can be centered are the rectangular faces parallel to the 2-fold axis. If we choose to call c the basis vector parallel to this axis, then the lattice mode can be A or Btype. If we choose to call it b, then it can be C or A-type. The orthorhombic lattice modes can be primitive (P), body-centered (I), face-centered (F), or base-centered A, B or C (generically, side-face centered, i.e. S), since the three faces can be centered. The triclinic, rhombohedral and hexagonal lattices can only be primitive. The rhombohedral lattice mode is usually noted R rather than P. The reason will be given in Chapters 5 (Sect. 5.6) and 6 (Sect. 6.3.3). The tetragonal lattice modes can be primitive (P) or centered (I), and the cubic lattice modes can be primitive (P), body-centered (I) or face-centered (F).

Chapter 3 – Crystal lattices

53

It can be shown that an F tetragonal lattice mode can be described via an I lattice mode (Exercise 3.10) and an F or I monoclinic lattice mode via an A or C lattice mode (Exercise 3.11), in full agreement with their absence among the Bravais lattice modes.

3.7.3. Reciprocal lattices of the non-primitive lattices We take as an example the face-centered cubic lattice, and search for its reciprocal lattice, the latter being deﬁned by starting from a primitive cell of the direct lattice. Let a, b, c be the basis vectors of the multiple (quadruple) cubic unit cell, and A, B and C the basis vectors of a primitive cell (Fig. 3.15a) such that A=

1 (b + c), 2

1 B = (c + a), 2

1 C = (a + b). 2

Let us denote the volume of this primitive cell by v0 , and let us determine the basis vectors A∗ , B∗ , C∗ of the reciprocal lattice, starting with A∗ . 1 1 (B × C) = [(c + a) × (a + b)] v0 4v0 1 [(c × a) + (c × b) + (a × b)]. = 4v0

A∗ =

(3.16)

Let a∗ , b∗ , c∗ be the basis vectors of the lattice reciprocal to the direct lattice for which the primitive cell would be the cube built on a, b and c. The volume (a, b, c) of this cubic unit cell of the direct lattice is 4v0 , so that 1 (b × c), 4v0 1 b∗ = (c × a), 4v0 1 (a × b). c∗ = 4v0 a∗ =

Equation (3.16) thus yields A∗ = b∗ − a∗ + c∗ . Similarly, we obtain B∗ = c∗ − b∗ + a∗ , C∗ = a∗ − c∗ + b∗ . If we build the reciprocal lattice starting from this primitive cell (A∗ , B∗ , C∗ ), we see that the lattice is body-centered cubic, the edges of the cube being the vectors 2a∗ , 2b∗ , 2c∗ (Fig. 3.15b). Note: the volume V ∗ of this body-centered cubic reciprocal unit cell is 8 times the volume v ∗ of the unit cell built on a∗ , b∗ and c∗ . Since v0 is the volume of

54

Symmetry and Physical Properties of Crystals

the primitive cell (the rhombohedron with angle 60◦ ), the volume of the unit cell built on a, b, c is 4v0 and the volume of its reciprocal cell (see Sect. 3.2.3) is v ∗ = 1/(4v0 ). We thus obtain V ∗ = 8v ∗ = 2/v0 . Since this reciprocal cell is body-centered, the volume of the primitive reciprocal unit cell is half this volume, i.e. 1/v0 as expected. The above derivation, which showed that the reciprocal lattice of a facecentered cubic lattice is a body-centered cubic lattice, was made on the basis of vector relations, without using the fact that the unit cell is cubic. The same derivation would apply for the orthorhombic face-centered lattice, and this would yield a body-centered reciprocal orthorhombic lattice. The orthorhombic reciprocal cell would have basis vectors 2a∗ , 2b∗ , 2c∗ if we again call the basis vectors of the direct orthorhombic cell a, b and c and those of the corresponding reciprocal lattice a∗ , b∗ and c∗ . The same approach shows (Exercise 3.13) that the reciprocal lattice of a bodycentered cubic lattice with basis vectors a, b and c is a face-centered cubic lattice with basis vectors 2a∗ , 2b∗ and 2c∗ . In the same way (Exercise 3.14), the reciprocal lattice of a base-centered lattice is shown to be a base-centered lattice.

3.8. Surface crystal lattice This section is related to a special area of crystallography: the study of surfaces. It is mandatory for whoever has any interest in investigating crystal surfaces. This research area developed considerably over the last years due to the importance of two-dimensional surfaces and interfaces in many phenomena such as catalysis, corrosion, the manufacturing of metal-semiconductor junctions, etc. To understand the mechanisms involved in these processes, the ﬁrst step consists in investigating plane surfaces with well-deﬁned crystal orientation and with low Miller indices, in order to determine their structure. The atoms located near the surface lose, due to the cut, some of their bonds. They must rearrange, together with their neighbors, in order to ﬁnd a new equilibrium position. This rearrangement can extend over several atomic layers near the surface. One then deﬁnes on the one hand the “bulk” of the crystal, with its three-dimensional periodic structure, and on the other hand the “surface”, which usually consists of several atomic layers, displaced with respect to their position in the bulk, and possibly with a diﬀerent stoichiometry. We also note that the study of surfaces is related not only to clean crystal surfaces, but also to the way foreign atoms, called adatoms, deposit on the surface. The “surface”, thus deﬁned as the set of atomic layers that are modiﬁed by the cut and possibly by the deposited adatoms, retains a two-dimensional periodicity. It is thus possible to deﬁne a surface crystal lattice. Determining this lattice is the ﬁrst step in an investigation of surfaces.

Chapter 3 – Crystal lattices

55

3.8.1. Cut surface Imagine we cut a crystal parallel to a given plane (hkl), and suppose the cut does not alter the atom positions. We can then determine a surface unit cell, deﬁned as the section of the crystal lattice in the bulk by a plane (hkl). This surface unit cell depends on the surface orientation. Consider the example of a primitive cubic lattice, with basis vectors a, b and c. For an (001) surface, the surface cell is square and has basis vectors a1 = a and b1 = b, while a (101) surface produces a rectangular surface cell with basis vectors a1 = a − c and b1 = b (Fig. 3.18a). Now consider a (101) surface in a body-centered lattice, then in a face-centered lattice. The surface unit cells are diﬀerent. If the bulk lattice is body-centered, the (101) surface unit cell is centered rectangular with basis vectors a1 = a − c and b1 = b (Fig. 3.18b). In the case of the face-centered bulk unit cell, the surface unit cell is simple rectangular, with basis vectors a1 = 1/2(a − c) and b1 = b (Fig. 3.18c). We thus determine easily a surface unit cell called the bulk-derived surface unit cell. We call a1 and b1 the basis vectors of this bulk-derived surface unit cell.

c

c

c b

b

a

b1

b

a

b1 a1

b1 a1

(a)

a

a1

(b)

(c)

Figure 3.18: Bulk-derived (101) surface unit cells in the (a) primitive cubic, (b) body-centered cubic and (c) face-centered cubic lattices

3.8.2. Real surface The existence of the surface alters the atom positions in the surface layer. If the displacements aﬀect only the direction perpendicular to the surface without altering the stoichiometry, the bulk-derived unit cell is retained at the surface. This case is referred to as relaxation of the atomic positions. However, surface atoms usually rearrange, thus altering the lattice unit cell at the surface. The surface is said to reconstruct. A simple case of rearrangement or reconstruction is that of the (101) surface of gold. Gold has in the bulk a face-centered cubic lattice. The crystal motif consists of one atom only, so

56

Symmetry and Physical Properties of Crystals

that Figure 3.18c can represent the atom positions in a unit cell. Figure 3.19a shows the atom positions which would prevail on the (101) surface if there were no reconstruction. The full circles correspond to the atoms in the ﬁrst layer, and the empty circles to the second layer. It so happens that the surface reconstructs so that the atoms of every other row parallel to the [10¯1] row in the ﬁrst layer disappear (Fig. 3.19b). This is described by saying that there is a missing row. The reconstructed surface unit cell, i.e. the unit cell of the real surface, then has as its basis vectors a2 = a1 = 1/2(a – c) and b2 = 2b1 = 2b. b2

b1 − [101]

a1

a2

(a)

(b)

Figure 3.19: Reconstruction of the (101) surface of gold. The full circles represent the positions of atoms in the ﬁrst layer, the empty circles those of the second layer and the gray ones those of the third layer. The upper part of each ﬁgure shows a top view; the lower part shows a cross-section. (a) The state of the surface if no reconstruction occurred. (b) Reconstructed surface, with its missing row parallel to [10¯1].

3.8.3. Notations The basis vectors (a2 , b2 ) of the real surface unit cell are generally expressed as a function of the basis vectors (a1 , b1 ) of the bulk-derived unit cell through the relations:

or

a2 = m11 a1 + m12 b1 , b2 = m21 a1 + m22 b1

a1 a2 =M . b2 b1

Matrix M deﬁnes the surface lattice completely. In the case of the (101) surface of gold which we just discussed, M is especially simple:

1 0 . 0 2 Another notation, due to Elizabeth A. Wood, is frequently used although it is not as general since it applies only to cases where: 1.

The angle between vectors a2 and b2 is the same as that between a1 and b1 .

Chapter 3 – Crystal lattices 2.

57

The lengths of a2 and b2 are expressed as a function of those of a1 and b1 by relations: a2 = p a1 and b2 = q b1 .

Noting ϕ the angle by which the surface lattice possibly has turned with respect to the bulk-derived lattice, the lattice for the (hkl) surface of a material with formula Y is indicated as: Y (hkl)(p × q)Rϕ. The simple case of the (101) surface of gold is thus described as Au (101) (1 × 2). We note that the rotation part is omitted if the lattice did not turn. In this notation, the bulk-derived cell is often designated as the (1×1) unit cell. Two examples of surface reconstructions where Wood’s notation can be used are shown on Figures 3.20 and 3.21. Figure 3.20 shows the reconstruction of a (001) surface of tungsten (W), cooled to below room temperature. This crystal is body-centered cubic with edge a, and the motif contains only one W atom. Figure 3.20a shows the atoms of this surface, as seen from above, if there were no reconstruction. The atoms in the ﬁrst layer are the empty circles, and those of the second layer are gray circles. The bulk-derived surface cell is a square with edges a and b, so that a1 = a and b1 = b. Due to the reconstruction, the ﬁrst layer atoms undergo a displacement along the arrows, thus creating, in a [1¯10] direction, a zigzag-like pattern, where the angle is no more 90◦ (Fig. 3.20b). The surface unit cell is a square (full lines on Fig. 3.20b), √ rotated by 45◦ with respect the bulk-derived cell, and its edge is a 2. It √ to √ is described as W (001) ( 2 × 2) R45◦ . It is sometimes described using the square face-centered cell (dotted lines) which is not rotated with respect to the bulk-derived cell, and it is then noted as c(2×2) with c standing for “centered”. b1 = b

a1 = a

(a)

(b)

Figure 3.20: Reconstruction of the W (001) surface. The empty circles represent the atoms of the ﬁrst layer, the gray circles those of the 2nd layer. (a) Bulk-derived cell. The arrows indicate the displacements which the atoms undergo during reconstruction. (b) Reconstructed surface and its primitive (full lines) and centered (dotted lines) unit cells. The second example deals with a surface covered with adatoms, the (111) surface of silicon (face-centered cubic lattice), covered with 1/3 of a monolayer of silver. The bulk-derived unit cell of a (111) surface of a fcc lattice is a hexagonal unit cell with basis vectors a1 = 1/2 [10¯1] and b1 = 1/2 [¯110]

58

Symmetry and Physical Properties of Crystals

represented on Figure 3.21a, where the atoms in the ﬁrst layer are full circles and those of the second layer are empty circles. The Ag atoms deposit above every third atom of the second layer, forming a regular lattice (large circles in thick lines in Fig. 3.21b). The surface unit cell is hexagonal, √ turned by 30◦ with respect to the bulk-derived cell, and the edge length is 3 times larger than the √ edge√of the bulk-derived hexagonal unit cell. It is described as Ag/Si (111) ( 3 × 3) R30◦ .

b1

a1 b2

(a)

a2

(b)

Figure 3.21: Reconstruction of a (111) surface of silicon covered with a third of a monolayer of silver. (a) Clean bulk-derived unit cell. The full circles represent the ﬁrst-layer atoms and the empty circles the secondlayer atoms. (b) Surface covered with Ag atoms, represented by large thick-line circles and located above second-layer atoms.

3.8.4. Reciprocal lattice Interpreting (X-ray or electron) diﬀraction by surfaces involves deﬁning a surface reciprocal lattice. It is therefore necessary to associate to the basis vectors of the surface unit cell a vector which is not in the surface plane. The appropriate vector is the smallest vector of the bulk crystal lattice perpendicular to the surface, and it is noted as n. a2 and b2 being the basis vectors of the unit cell of an (hkl) surface, the reciprocal lattice of the unit cell (a2 , b2 , n) is then deﬁned by the vectors a∗2 , b∗2 , n∗ such that a∗2 = b∗2 = n∗ =

b2 × n , V n × a2 , V a2 × b2 . V

V , the volume built on vectors a2 , b2 and n, is such that V = n · (a2 × b2 ). We note that the vector n∗ is perpendicular to the surface and its norm is equal to the reciprocal of the norm of vector n. For the reconstructed surfaces discussed above, the relevant vectors n are: 1 surface Au (101) (1 √ × 2)√: n = /◦2 [101], surface W (001) ( 2 √ × 2)√R45 : n = [001], surface Ag/Si (111) ( 3 × 3) R30◦ : n = [111].

Chapter 3 – Crystal lattices

59

3.9. Exercises Exercise 3.1 1.

Determine the indices (hkl) of the plane that goes through the three nodes (1, 0, 0), (0, 1, 0) and (0, 0, 3).

2.

Show that the three rows [211], [120] and [302] are coplanar. What are the indices of their common plane?

3.

Determine the row common to the planes (311) and (1¯10).

Exercise 3.2 Titanium oxide TiO2 has a tetragonal lattice with parameters a = 4.59 Å and c = 2.96 Å. 1.

What is the angle between faces (101) and (10¯1)?

2.

Show that, in this system, row [hk0] is perpendicular to plane (hk0), but that the same does not apply to row [0kl] and plane (0kl).

3.

Calculate the lattice distance of planes (321).

Exercise 3.3 1.

Consider a plane crystallographic lattice with basis vectors a and b. We choose an axis system Oxy parallel to a and b, with unit lengths a and b respectively. Consider the row D that goes through points M and N, with coordinates respectively (2, 0) and (0, 3). Determine: (a) the equation of row D. (b) the number of rows parallel to D located between D and the origin O of the lattice. (c) the equations of the rows belonging to this family that go through the point with coordinates (1, 0) and (0, 1) respectively.

2.

Consider the three-dimensional crystallographic lattice with basis vectors a, b as given in (1) and c, where c is a general lattice vector which does not belong to plane (a, b). (a) Determine the values of h, k and l for the family (hkl) of lattice planes parallel to vector MN and c. (b) Determine the values of h, k and l for the family (hkl) of lattice planes parallel to the plane that goes through MN and through the point P with crystallographic coordinates (0, 0, 1).

60

Symmetry and Physical Properties of Crystals

Exercise 3.4 Hexagonal lattice: we recall that the basis vectors a, b and c of the unit cell are such that a = b = c and that the angles are α = β = 90◦ and γ = 120◦ . 1.

Determine the reciprocal lattice of the hexagonal lattice, and give its orientation with respect to the direct lattice.

2.

Calculate the length of the vector [110]∗ of the reciprocal lattice. Deduce the value of the lattice distance between (110) planes. Retrieve this result through a geometrical argument without using the reciprocal lattice.

3.

Calculate the angle between planes (120) and (100).

Exercise 3.5 Consider a hexagonal lattice. The plane (hkil) closest to the origin of the lattice intersects plane (a, b) along a line which intersects vector a at point M such that OM = a/h, vector b at point N such that ON = b/k and vector d at point Q such that OQ = d/i. Vector d is deduced from b through a rotation by 120◦ around c. Draw a ﬁgure in plane (a, b) and note that a + b + d = 0. 1.

Express the area of triangles OMN, OMQ and OQN as a function of the cross product of two of the basis vectors a, b or d.

2.

By writing that the area of OMN is the sum of the areas of OMQ and OQN and by substituting for d its value as a function of a and b, show that you obtain the relation h + k + i = 0.

3.

Consider the (1 2 3 1) lattice plane family. Determine the lattice plane family which deduces from it through a rotation by 2π/3, then the family obtained through a rotation by 4π/3. In the same way, determine the families of planes obtained through symmetry with respect to plane (a, c) and with respect to plane (b, c) respectively.

Exercise 3.6 Show that the set of points consisting of the nodes of a crystal lattice and the points at the centers of four pairwise parallel faces of the unit cell, do not form a crystal lattice. In other words, a crystal lattice cannot have two distinct faces that are centered. Note that crystal periodicity implies that every face deduced through a lattice translation from one that is centered must also be centered. Exercise 3.7 Consider the crystal structures, with cubic lattice, shown on Figures 8.3 (CsCl, NaCl, ZnS) and 8.6 (diamond). Determine their Bravais lattice and their motif. Same question for the structures of Figure 8.4: cubic CaF2 , tetragonal TiO2 and cubic CaTiO3 .

Chapter 3 – Crystal lattices

61

Exercise 3.8 Consider the structure of graphite shown on Figure 8.11. 1.

Draw a projection onto the plane of the hexagons, indicating their heights, of the atom positions. Take as a unit twice the distance between two neighboring carbon planes.

2.

Determine the unit cell, its parameters using the data shown on Figure 8.11, and the number of atoms per unit cell.

Exercise 3.9 The structure of a compound consisting of nickel and gadolinium can be represented as follows. Decompose space into a set of identical right prisms, with regular hexagons as their bases, and contacting one another. Each apex and each center of the lateral faces of the prism is occupied by a nickel atom. The Gd atoms are located at the centers of the hexagonal bases of the prism. In the basal plane, the shortest Ni–Gd distance is 2.83 Å and the height of the prisms is 3.97 Å. 1.

Determine the chemical formula of this compound.

2.

Draw a projection of the atom positions onto the basal plane, stating the heights, and deduce the lattice and the motif.

3.

With the lattice now deﬁned, give the Miller indices of the prism faces.

4.

Calculate the angle between planes (1¯10) and (110).

Exercise 3.10 Show that a tetragonal F (face-centered) lattice mode can be described by a tetragonal body-centered unit cell (I type lattice mode) with half the volume. It will be useful to make a projection of the lattice nodes onto a plane perpendicular to the basis vector c, mentioning the heights. Exercise 3.11 Show that a monoclinic F lattice mode can be described by a monoclinic I lattice mode with a unit cell half the volume, and that this I lattice mode can be described by a base-centered monoclinic unit cell with the same volume. It will be useful to draw a projection of the lattice nodes onto the plane normal to the 2-fold axis of the initial monoclinic lattice, specifying the heights. Exercise 3.12 Draw a projection onto the plane (111) of the nodes of a cubic F lattice, indicating the heights. Show that this yields a ﬁgure similar to Figure 3.14c. Use the fact that direction [111], parallel to a major diagonal of the cube, is a 3-fold axis for the (111) planes which are perpendicular to it.

62

Symmetry and Physical Properties of Crystals

Exercise 3.13 Consider a body-centered cubic lattice with basis vectors a, b and c. Let A, B and C be the basis vectors of the primitive rhombohedral unit cell: 1 A = (b + c − a), 2

1 B = (c + a − b), 2

1 C = (a + b − c). 2

Call a∗ , b∗ and c∗ the basis vectors of the reciprocal unit cell of a primitive cubic unit cell with basis vectors a, b and c. 1.

Determine the basis vectors A∗ , B∗ and C∗ of the reciprocal lattice as a function of A, B and C, then as a function of a∗ , b∗ and c∗ .

2.

Show that the reciprocal lattice of the body-centered cubic unit cell with basis vectors A∗ , B∗ and C∗ is a face-centered cubic lattice with basis vectors 2a∗ , 2b∗ and 2c∗ .

Exercise 3.14 Consider any base-centered lattice, for example A-type, with basis vectors a, b and c. Choose as basis vectors of the primitive unit cell the vectors A = a,

1 B = (b − c), 2

1 C = (b + c). 2

Let a∗ , b∗ and c∗ be the basis vectors of the reciprocal unit cell of a primitive lattice, with basis vectors a, b and c. Show that the reciprocal lattice of the A-type base-centered lattice is a basecentered A-type lattice with basis vectors a∗ , 2b∗ and 2c∗ .

Chapter 3 – Crystal lattices

63

Appendix 3A. The metric tensor The metric tensor is particularly useful for numerical calculations.

3A.1. Deﬁnition The term tensor will be explicitly deﬁned and discussed in Chapter 9, but the formal deﬁnition is not needed here. The term metric means it deals with measure, here the lengths and angles between the basis vectors of the crystal unit cell. The components of the metric tensor are deﬁned by the dot products of the basis vectors of the unit cell, which we note as a1 , a2 and a3 , i.e. the ai with i ranging from 1 to 3, so that gij = ai · aj . The metric tensor is also deﬁned in reciprocal space: ∗ gij = a∗i · a∗j .

3A.2. Volume of the unit cell The volume V of the direct unit cell is: V = a1 · (a2 × a3 ) = (a1 , a2 , a3 ). We express the basis vectors of the unit cell in an orthonormal basis {e1 , e2 , e3 }: a1 =

3

B1j ej

j=1

which can be written using Einstein’s convention, deﬁned in Section 9.3.1. Einstein’s convention consists in suppressing the summation sign (which becomes implicit) in a product of factors when the subscript over which the summation is to be performed is repeated. Thus we can write a1 = B1j ej . Since the subscript j appears twice, it is clear that summation must be performed over j. In a similar way, we write for each of the basis vectors ai : ai = Bij ej . It is easy to check that (a1 , a2 , a3 ) = det B (e1 , e2 , e3 ) where det B is the determinant of the matrix {Bij } or B matrix.

64

Symmetry and Physical Properties of Crystals

Since the basis {e1 , e2 , e3 } is orthonormal, its volume is equal to 1, hence V = det B,

(3A.1)

gij = ai · aj = Bik ek · Bjl el = Bik Bjl ek · el = Bik Bjl δkl = Bik Bjk .

(3A.2)

T where B T is the transposed matrix of B. Bjk can be substituted by Bkj T , so that g = BB T if we call g the matrix {g }, and We obtain gij = Bik Bkj ij

det g = det B det B T = (det B)2

(3A.3)

since the determinants of a matrix and of its transpose are equal. Comparing (3A.1) and (3A.3), we see that V 2 = det g.

(3A.4)

It is on the basis of this formula that, in Section 3A.5 below, the volume of the triclinic unit cell will be easily calculated.

3A.3. Product of the matrices associated to the direct and reciprocal metric tensors ∗ = a∗ · a∗ , where The reciprocal metric tensor is deﬁned by the coeﬃcients gij i j ∗ the ai (i = 1 to 3) are the basis vectors of the reciprocal unit cell.

Let us express the vectors a∗i in the direct basis {a1 , a2 , a3 }: a∗i = Mik ak and

∗ gij

=

a∗i

·

a∗j

= Mik ak · a∗j = Mik δkj = Mij

since the reciprocal lattice vectors are deﬁned by relations (3.4), which can be written: a∗i · ak = δik where δik is Kronecker’s symbol, equal to 1 if i = k and equal to 0 otherwise. Using ∗ a∗i · ak = Mij aj · ak = Mij gjk = gij gjk ,

we obtain ∗ gjk = δik . gij

This relation shows that the product of the matrices g and g∗ is equal to the unit matrix E gg ∗ = E.

(3A.5)

Chapter 3 – Crystal lattices

65

The calculation of the reciprocal metric tensor is therefore performed by inverting the matrix associated to the direct metric tensor. Taking the determinant of both sides of Equation (3A.5), we obtain: det g det g∗ = 1. It can be shown that det g∗ = (V ∗ )2 , as was done for the volume of the direct unit cell, and we retrieve the fact that the volume of the reciprocal unit cell is equal to the reciprocal of the volume of the direct unit cell.

3A.4. Calculation of lattice distances The lattice distance of a family of planes (hkl) is given by relation (3.8): dhkl =

1 1

=

hi a∗ . h∗ i

∗ and We can write hi a∗i 2 = (hi a∗i ) · (hj a∗j ) = hi hj gij

dhkl =

1 ∗ hi hj gij

(3A.6)

which is easily calculated knowing the reciprocal metric tensor which is calculated by inverting matrix g (Eq. (3A.5)).

3A.5. Applications The metric tensor can be written, with the usual notations for the parameters of the crystal lattice: ⎞ ⎛ ab cos γ ac cos β a2 bc cos α ⎠ . b2 g = ⎝ ab cos γ ac cos β bc cos α c2 The determinant of this matrix is given by det g = a2 b2 c2 (1 − cos2 α − cos2 β − cos2 γ + 2 cos α cos β cos γ) whence we deduce through (3A.4) the volume V of the unit cell: V = abc 1 − cos2 α − cos2 β − cos2 γ + 2 cos α cos β cos γ. Inverting matrix g leads to matrix g∗ , so that ⎛ 2 2 2 ⎞ b c sin α abc2 Kαβγ ab2 cKγαβ 1 g∗ = 2 ⎝ abc2 Kαβγ a2 c2 sin2 β a2 bcKβγα ⎠ V ab2 cKγαβ a2 bcKβγα a2 b2 sin2 γ where we use the temporary notation cos α cos β−cos γ = Kαβγ , with two other coeﬃcients Kβγα and Kγαβ being obtained through a circular permutation of the subscripts.

66

Symmetry and Physical Properties of Crystals

Since g∗ is a symmetrical matrix, the general expression (3A.6) of dhkl is given by dhkl =

1 ∗ h2 + g ∗ k 2 + g ∗ l2 + 2g ∗ hk + 2g ∗ hl + 2g ∗ kl g11 22 33 12 13 23

and, in the most general case of the triclinic unit cell, we obtain: 1 − cos2 α − cos2 β − cos2 γ + 2 cos α cos β cos γ dhkl = A with h2 k2 l2 hk sin2 α + 2 sin2 β + 2 sin2 γ + 2 (cos α cos β − cos γ) 2 a b c ab hl kl + 2 (cos α cos γ − cos β) + 2 (cos β cos γ − cos α) ac bc

A=

Chapter 4

Relationship between space groups and point groups After showing that the symmetry operations of a crystal form a group, we show how to go over from this group to the space group characterizing the crystal structure on the microscopic scale, and then to the point group, which governs its macroscopic physical properties. The rigorous proof is preceded by an example which allows the reader to grasp these notions intuitively.

4.1. Introduction The most general symmetry operation which any object, and in particular a crystal, can have can be noted [S(O), t] where S represents a rotation or a rotoinversion (deﬁned in Sect. 2.1) whose axis goes through point O, and t a translation. In the case of rotoinversion, O is also the associated symmetry center. Note that point O, which deﬁnes the position of the axis, has no reason not to change from one operation to another. We will show in the next section that the symmetry operations [S(O), t] of the crystal make up a group. Among all these symmetry operations, there is the set of lattice translations T, and it is interesting to consider the symmetry operations [S(O), t] modulo the lattice translations. The expression “[S(O), t] modulo the lattice translations” means that we do not distinguish operations [S(O), t] and [S(O), t+n] if n is any lattice vector (n belonging to T). It will be shown that these operations form a group, called the position group or space group of the crystal. Consider the direction of a straight line in the crystal, parallel to a vector D, and submit it to any one of these symmetry operations. It becomes another straight line, parallel to vector D such that D = [S(O), t] D = S(O) D = S D

(4.1)

because D is unaltered by any translation t. Reference to point O was suppressed because the result D does not depend on the position of the rotation axis, nor on the point on the axis which is used for inversion when the operation

© Springer Science+Business Media Dordrecht 2014 C. Malgrange et al., Symmetry and Physical Properties of Crystals, DOI 10.1007/978-94-017-8993-6_4

67

68

Symmetry and Physical Properties of Crystals

is a rotoinversion. The only relevant data are the direction of the axis and the rotation angle. Since D is deduced from D through a symmetry operation of the crystal, the macroscopic properties measured along directions D and D will be the same (for example, the elongation of a bar parallel to D or to D under the inﬂuence of a given increase in temperature). We thus understand that the symmetry of the macroscopic properties of the crystal is governed by the operations S solely deﬁned by the direction of a rotation (or rotoinversion) axis and the rotation (or rotoinversion) angle. We will show in Section 4.3 that these operations S comprise a group, called the orientation group of the crystal or the point group. The latter term reminds us that, for this group, all the symmetry elements can be made to go through a given point, since the position of the symmetry element does not matter. The point group is thus obtained from the space group of the crystal by ignoring all translations (or, equivalently, by replacing all translations with the zero translation), and by having all the rotation or rotoinversion axes go through one given point, which will also be the center of symmetry used if there is a rotoinversion. In order to illustrate the notions of space group and point group, consider the plane periodic ﬁgures of Figure 4.1, which we assume to extend to inﬁnity. They can be considered as sorts of two-dimensional crystals. Figure 4.1a (the crystal lattice of which is shown in Fig. 4.1b) features two families consisting of an inﬁnity each of mirrors, parallel to one another and perpendicular to the plane of the ﬁgure. The mirrors of one of the families are denoted as Mi and the symmetry operation associated to mirror Mi is designated as mi (symmetry with respect to plane Mi ). The mirrors of the other family, perpendicular to the mirrors Mi , are denoted as Mj and the associated symmetry operations as mj . The symmetry operations of this plane crystal have the form [mi , ua+vb] and [mi , u a+v b],1 where u, v, u and v are integers and a and b are the basis vectors of the lattice. We must add to these operations the products of these operations. These product operations are rotations by 180◦ , denoted Rk , around axes perpendicular to the plane lattice, located at the intersections of the mirrors, followed by lattice translations, hence [Rk , u a + v b]. We will show (Exercise 4.1 and Sect. 7.2.2) that the product of a mirror operation m (symmetry with respect to a mirror plane M) by a translation t perpendicular to the mirror is a pure mirror operation where the new mirror is deduced from M by a translation t/2. We thus obtain: [m1 , b] = [m2 , 0];

[m1 , 2b] = [m3 , 0];

[m1 , −b] = [m0 , 0];

etc.

(4.2)

¯ axis normal to the mirror 1. Here we simpliﬁed the notation. A mirror is equivalent to a 2 for which the reference symmetry center is located at the point where the axis intersects the mirror. The notation consistent with [S(O), t] would, for operation (mi , ua +vb) (see Sect. 4.2.1), be [¯ 2(Oi ), ua + vb], with point Oi located at the intersection of the ¯ 2 axis with the plane Mi .

Chapter 4 – Relationship between space groups and point groups

69

M’0 M’1 M’2 M3 M2 M1 M0

b

M–1

a

(b)

(a) M’1

O’ a/2

O

M1 b a

(c)

(d)

Figure 4.1: Examples of plane “crystals” (a) and (c) and their crystal lattices (b) and (d) The mirror operations [m1 , vb] with v an integer thus describe the set of operations [mi , 0]. The set of operations [mi , ua+vb] can thus be replaced by the set [m1 , ua+vb] where m1 is the operation associated to any one particular mirror chosen as the reference (here M1 ), and u and v any integers. This set of symmetry operations, modulo the lattice translations T, can be represented by operation [m1 , 0]. The same reasoning applied to operations [mj , u a + v b] modulo T shows that [m1 , 0] can represent the set of operations [mj , u a + v b] modulo T and that [R1 , 0] can represent the set of operations [Rk , u a + v b] modulo T. The symmetry operations of this crystal, modulo the lattice translations T, are thus identity, a mirror operation m1 , a mirror operation m1 , and operation R1 , a rotation by π around the intersection of the mirrors M1 and M1 . This is a set Gs such that: Gs = [E, 0] + [m1 , 0] + [m1 , 0] + [R1 , 0] modulo T. These symmetry operations make up the space group. The point group G0 , obtained by deleting all translations and having all the symmetry elements go through the same point, is thus: G0 = [E, 0] + [m1 , 0] + [m1 , 0] + [R1 , 0]. Now consider the “crystal” of Figure 4.1c, whose lattice, shown on Figure 4.1d, is identical to that of Figure 4.1a. It also features two families of mirrors, but the mirrors of family Mi are glide mirrors (Sect. 2.2.4), the symmetry operation of which is the product of operation mirror mi and of translation a/2.

70

Symmetry and Physical Properties of Crystals

The symmetry operations of this crystal have the form [m1 , (u + 12 )a + vb], [m1 , u a + v b] and their products. The mirror operations of the space group are now [m1 , a/2] and [m1 , 0] modulo the lattice translations. The space group is thus: Gs = [E, 0] + [m1 , a/2] + [m1 , 0] + [R , 0] modulo T. Operation R is a rotation by 180◦ around the axis intersecting the plane of the ﬁgure at point O deduced from O, the intersection of the traces of M1 and M1 , through translation a/4 (Exercise 4.2). The point group G0 is obtained from Gs by suppressing all translations and having all the symmetry elements go through one single point. We obtain: G0 = [E, 0] + [m1 , 0] + [m1 , 0] + [R1 , 0]. The two “crystals” we are discussing have diﬀerent space groups but the same point group G0 . Further in this chapter, we will show rigorously how to go over from the group of symmetry operations which the crystal features, to its space group, and from the space group to the point group. This will require the use of the quotient group notion. It is deﬁned in Appendix 4A, a refresher on some properties of groups which may be useful reading. However, the reader may be content, on a ﬁrst quick reading, with the approach just given. It provides a feeling for the point group and space group notions and their relationship. The reader can then go over directly to the next chapter, Chapter 5, which lists in a logical way the various point groups which crystals can feature.

4.2. Symmetry operations of the crystal 4.2.1. Change in origin A symmetry operation [S(O), t] transforms point M1 into point M2 such that OM2 = S(OM1 ) + t. Let us show that we can change origin, i.e. ﬁnd S , O and t such that [S (O ), t ] = [S(O), t]. O M2 = S (O M1 ) + t

Then

(4.3)

for any M1 . Let us explicit both sides of Equation (4.3). O M2 = O O + OM2 = O O + S(OM1 ) + t.

(4.4)

S (O M1 ) + t = S (O O + OM1 ) + t = S (O O) + S (OM1 ) + t .

(4.5)

Chapter 4 – Relationship between space groups and point groups

71

Since the right hand sides of Equations (4.4) and (4.5) are equal, we deduce that S(OM1 ) + t = S (OM1 ) + S (O O) − O O + t which must be true for any point M1 . This implies that: S = S,

(4.6)

t = t + (S − E)(OO )

(4.7)

where E is the identity operation. We can therefore replace all the symmetry operations [S(O), t] featured by the crystal with operations [S(O ), t ] where O is now common to all the symmetry operations, provided each translation t is replaced by translation t given by Equation (4.7). We can thus choose a reference point common to all the symmetry operations, hence simplify the notation by not mentioning this reference point. This will be done throughout the remainder of this chapter. We denote as (S, t) the symmetry operations featured by a crystal, with the understanding that a point O common to all the symmetry operations of the crystal has been chosen. We now show that these operations form a group, the symmetry group of the crystal.

4.2.2. The operations (S, t) form a group The product of two symmetry operations of a crystal is of course also a symmetry operation. Let us look for the expression of the product of two of these operations, viz. (S1 , t1 ) which changes M into M1 and (S2 , t2 ) which transforms M1 into M2 . OM1 = S1 (OM) + t1 OM2 = S2 (OM1 ) + t2 = S2 S1 (OM) + S2 t1 + t2 whence

(S2 , t2 )(S1 , t1 ) = (S2 S1 , S2 t1 + t2 ).

(4.8)

Search for the neutral element: by using relation (4.8), we easily check that the neutral element is (E, 0) where E is the identity operation. The proof is (E, 0)(S, t) = (S, t)(E, 0) = (S, t). Search for the inverse element: we want to determine (S, t)−1 = (S , t ) such that (S , t )(S, t) = (E, 0). From (4.8), (S , t )(S, t) = (S S, S t + t ) hence S S = E and S t + t = 0. Therefore

S = S−1 , t = −S−1 t.

(4.9)

72

Symmetry and Physical Properties of Crystals

S−1 is the inverse operation of S. Consider an example: if S is a rotation by 2π/3 around a given axis (which goes through the point O common to all the symmetry operations), S−1 is a rotation by −2π/3 around the same axis. The translation t is the opposite of the vector deduced from t through a rotation by −2π/3 around the axis (Fig. 4.2). M’

M1

t

S −1(t)

M

O

t’ = −S −1(t) M’1

Figure 4.2: Illustrating the inverse operation of (S, t), where S is the rotation by 2π/3 around an axis perpendicular to the plane of the ﬁgure and going through O. M1 is the transform of M under this operation. The rotation by −2π/3 around the same axis transforms M1 into M1 , and translation t = − S−1 t brings M1 back to M.

4.2.3. The lattice translations form an invariant subgroup of the group of symmetry operations of the crystal To prove this result and that of the next section, we use a few deﬁnitions and properties of invariant subgroups and of quotient groups given in Appendix 4A. The lattice translations are the symmetry operations (E, n) where E is the identity operation and n = ua + vb + wc, a, b and c are the basis vectors of the unit cell and u, v, w are integers. We show that the set of operations (E, n) form a group, which is a subgroup of the symmetry operations (S, t) of the crystal. The product of two lattice translations is a lattice translation, and the neutral element (E, 0) is part of this set. Let us show that this subgroup is invariant (Appendix 4A), i.e. that, for any S, we have: (S, t)(E, n)(S, t)−1 = (E, n ). (S, t)(E, n)(S, t)−1 = (S, t)(E, n)(S−1 , −S−1 t) = (S, t)(S−1 , −S−1 t + n) = (E, −SS−1 t + Sn + t) = (E, Sn). (E, Sn) is a pure translation. It is a symmetry operation of the crystal since it was obtained as the product of symmetry operations of the crystal. Since its rotation part is identity, it is necessarily a crystal lattice translation.

Chapter 4 – Relationship between space groups and point groups

73

Conclusion 1.

The set of lattice translations is an invariant subgroup of the group of the symmetry operations of the crystal.

2.

We showed that Sn is a crystal lattice vector. This result shows that the operations S are symmetry operations of the lattice. We will see at the end of Section 4.3 that the reciprocal proposition is not necessarily true.

4.3. Space groups and point groups The subgroup (E, n) = T of the lattice translations being invariant, we can deﬁne a quotient group G/T starting from the partition of G by T (Appendix 4A). The partition of G into cosets products of T by symmetry operations of the crystal which are not lattice translations can be expressed as G = T + T(S1 , t1 ) + T(S2 , t2 ) + T(S3 , t3 ) + . . . + T(Sm , tm ). This partition is performed in the following way: we isolate within G a ﬁrst packet of operations, here the lattice translations T. Among the remaining operations, we choose an operation (S1 , t1 ). We perform the product of this operation by all the lattice translations, forming the second packet T(S1 , t1 ), and so forth until all the elements of G have been used. We here operate with the smallest possible vectors (null or smaller than a lattice vector) by subtracting from the initial translation vector tj as large a lattice vector ni as possible. This lattice vector ni may then be included in T. This is possible since (Si , tj ) = (Si , ti + ni ) = (E, ni )(Si , ti ) so that

T(Si , tj ) = T(Si , ti ).

We will determine further (Sect. 7.2) the symmetry operations (Si , ti ), where ti is a non-zero vector smaller than a crystal lattice vector, which may exist in a crystal. We will see that they are the symmetry operations associated to screw axes or to glide mirrors (Sect. 7.2.1 and 7.2.2). The quotient group is deﬁned as Gs = G/T, the group whose elements are the cosets T(Si , ti ). If we consider the symmetry operations modulo T, we can replace coset T(Si , ti ) by (Si , ti ). We can then write Gs = (E, 0) + (S1 , t1 ) + (S2 , t2 ) + (S3 , t3 ) + . . . + (Sm , tm ) modulo2 T. In the introduction to this chapter, we deﬁned two operations equivalent modulo T as two operations for which the diﬀerence in the translation parts 2. Adding “modulo T” is mandatory in order for the above operations to form a group because it can happen that the product of two of the operations (Si , ti ) is equal to (Sj , tj + n) while, as mentioned above, the ti are smaller than lattice translations.

74

Symmetry and Physical Properties of Crystals

is equal to a lattice translation n. (E, n)(S, t) = (S, t + n).

This is indeed the case here since

Gs is called the space group, or position group, of the crystal. Now consider the operations (E, 0), (S1 , 0), (S2 , 0), etc. which deduce from the elements of Gs by canceling all the translations, i.e. by canceling the “modulo T” and replacing the ti by 0. Using the composition law (4.8), it is easy to show that these operations form a group G0 , isomorphous to Gs , which can be written G0 = (E, 0) + (S1 , 0) + (S2 , 0) + (S3 , 0) + . . . + (Sm , 0). This group is the point group (or orientation group) of the crystal. It is obtained by considering all the symmetry operations of the crystal, deﬁned, as we remember, with a common origin (Sect. 4.2.1), and by canceling all translations. We saw, at the end of Section 4.2.3, that the operations (Si , 0) are symmetry operations of the lattice. The reciprocal proposition is not necessarily true (and indeed it is often wrong), i.e. all symmetry operations of the lattice are not necessarily symmetry operations of the point group. We note that: The symmetry operations of the point group of the crystal form a subgroup of the symmetry operations of the crystal lattice. A simple example, chosen from among the plane lattices, is given on Figure 4.3a. The crystal features a family of pure plane mirrors Mi , and does not feature any mirror perpendicular to the Mi . The point group of the crystal is G0 = (E, 0) + (m, 0) where m is the symmetry operation associated to one of the mirrors Mi . M3 M2 M1 M0

b

M–1

(a)

Figure 4.3: lattice in (b)

a

(b)

(a) An example of a plane “crystal”, with its crystal

The crystal lattice (Fig. 4.3b), for which the unit cell is a rectangle, features a family of mirrors Mi perpendicular to the Mi . Let us denote with m the symmetry operation associated to one of the mirrors Mi , and with A the product of operations m and m , i.e. the rotation by π around their intersection. The point group of the crystal lattice is G0 = (E, 0) + (m, 0) + (m , 0) + (A, 0)

Chapter 4 – Relationship between space groups and point groups

75

and indeed G0 is a subgroup of G0 . As was discussed at the beginning of this chapter, the point group of the crystal is very important because it governs the symmetry of the macroscopic properties of crystals. Furthermore, the construction of space groups is easy to explain when starting from the point groups. We therefore start by investigating the point groups or orientation groups (Chap. 5) and then, in Chapter 7, we show how the space groups or position groups can be built starting from the point groups. For a given point group, it is useful to know the directions that are equivalent to a given direction through the symmetry operations which are elements of the group. These equivalent directions are represented using the stereographic projection, deﬁned in the next chapter.

4.4. Exercises Exercise 4.1 Show that the product of a symmetry with respect to a plane P and a translation by a vector V perpendicular to plane P is a symmetry with respect to the plane P deduced from P by a translation V/2. Consider a general point M, its image M1 by symmetry with respect to P, and then the point M2 , image of M1 through translation V. Draw the ﬁgure in the plane Π perpendicular to P and going through M. Exercise 4.2 1.

Show that the product of a symmetry with respect to a plane P1 and a symmetry with respect to a plane P2 perpendicular to P1 is a rotation by π around zz , the intersection of planes P1 and P2 .

2.

Now replace the second symmetry operation of (1) by the operation product of the symmetry with respect to P2 and a translation V perpendicular to zz and parallel to plane P2 . Show that this ﬁnal operation is a rotation by π around an axis deduced from zz through a translation V/2.

76

Symmetry and Physical Properties of Crystals

Complement 4C. Probes used for crystal structure determination 4C.1. Possible probes and criteria for choice Crystal structure research mainly involves the determination of the nature of the atoms comprising the material and their arrangement in space. This process is invariably based on coherent scattering, i.e. diﬀraction. It therefore requires probes that interact with atoms, with a wavelength smaller than the distances between atoms, viz. 1 Å = 1 ×10−10 m = 0.1 nm. The wavelength is given by λ = h/p where h is Planck’s constant h = 6.63 ×10−34 J s and p the probe momentum. There are three possibilities: X-rays, neutrons and electrons. Electrons can be eﬀectively focused through magnetic lenses, giving the possibility of either imaging or diﬀraction modes in the electron microscope. Neutrons and X-rays can be focused, either by reﬂection from curved mirrors or crystals, or through diﬀractive lenses (zone plates, or Fresnel lenses), or through the use of refractive lenses consisting of stacks of small spheres or paraboloids, or holes in materials. Much better results are obtained in the case of spatially coherent beams of synchrotron X-rays3 . These three probes interact with diﬀerent features of matter. X-rays interact with the electrons within materials, stronger scattering being associated with atoms with more electrons, i.e. with heavier atoms. Neutrons are sensitive to the nature of the nuclei (number of protons, i.e. chemical nature, but also number of neutrons, hence isotope) and also to the magnetic ﬁelds within matter. Electrons sense the electrostatic potential due to both the nuclei and the electrons. In structural work, the fact that there is no systematic relation between the strength of nuclear scattering (the nuclear scattering length) of thermal neutrons and the atomic number of the scatterer opens up possibilities for elegant approaches complementary to X-ray diﬀraction. Electrons are strongly absorbed by materials, and can go through thin samples only (typically less than 1 micrometer), while X-rays, and even more neutrons, can go through thick samples. These probes are also very diﬀerent in their ease of production and in the intensity of the beams that can be obtained. The probe with by far the widest use is X-rays.

4C.2. X-rays X-rays are electromagnetic waves. They have the proper range of wavelength λ, around 1 Å, when their photon energy E = hc/λ where c is the velocity of light in vacuum, is of the order of 10 keV. They are produced, like all electromagnetic waves, when light electric charges (in eﬀect electrons) are accelerated. The standard sources for X-rays are laboratory X-ray tubes, in which electrons are accelerated by a voltage V on the order of 104 V and hit a metal target, the anode. X-rays are emitted both in the form of “character3. Christian David, http://www.psi.ch/lmn/x-ray-optics

Chapter 4 – Relationship between space groups and point groups

77

istic” radiation, i.e. fairly ﬁne spectral lines, and in the form of a continuous spectrum, Bremsstrahlung.4 The characteristic lines correspond to transitions of atomic electrons between discrete atomic energy levels as the electron vacancies induced by the incoming electrons heal, and their energies or wavelengths depend on the target material. X-rays are also produced, with much higher intensity than in laboratory X-ray tubes, as part of the synchrotron radiation emitted when the trajectories of ultra-relativistic electrons or positrons (energy E much larger than their rest mass energy me c2 = 0.511 MeV) are curved by a magnetic ﬁeld. Synchrotron radiation covers a huge spectral range, from the infrared, through the visible and ultra-violet range, to high-energy X-rays if the energy of the electrons or positrons is high enough, and it is the hard X-ray part (typically 10 to 100 keV energy, or about 0.1 to 0.01 nm wavelength) that is put to use for structural work. Monochromatic beams (beams with a given energy or wavelength) must be prepared through monochromators. In practice, synchrotron radiation sources are storage rings into which the particles are fed after being accelerated to energies of several GeV. Initially considered by high energy physicists as a nuisance, synchrotron radiation is now the sole motivation for the construction of “dedicated” machines. Beyond intensity, synchrotron radiation oﬀers, among the features useful in structure determination, the possibility of tuning the wavelength, and in particular of aiming for selected values where the response of one given type of atoms is enhanced by resonance. For most structure investigations, laboratory X-rays, obtained from X-ray generators which are aﬀordable for normal size laboratories, are satisfactory; access is then easy for the researchers. In some special cases, higher intensity or other requirements make it desirable to use hard X-rays from synchrotron radiation sources. These large facilities, with high construction and operation cost, are mostly available in developed countries. For example, in 2011, APS (Advanced Photon Source) in the USA, Spring8 in Japan and ESRF in Europe, Diamond the British source, Petra III the new German source, Swiss Light Source (SLS), Soleil the French one, all are third-generation, i.e. highest-performance sources. They are accessible to researchers on the basis of applications for beam-time which are ranked by committees, a procedure which takes time – and does not always lead to acceptance. Thus their use is eﬀectively reserved for work, much of which is outside structural crystallography, which cannot be performed with laboratory X-rays. Novel large facilities for the production of X-rays are appearing: free electron lasers or XFEL (X-ray Free Electron Lasers). They produce pulses of coherent X-rays with extremely large intensity and a duration of less than 100 femtoseconds. This makes it possible to envisage watching atomic movements in solids, understanding chemical reac4. Bremsstrahlung (with a capital B ) is the German word for “radiation from braking”. It is associated with the decrease in velocity of electrons through interaction with the target material. Energy conservation immediately yields a useful feature: the energy of a photon cannot be more than that of the electrons, thus the short-wavelength limit of the spectrum is such that hc/λmin = eV .

78

Symmetry and Physical Properties of Crystals

tion processes on the molecular scale, etc. Two such sources are operational in 2011: LCLS (Linac Coherent Light Source) at Stanford, CA, USA since 2009, while SACLA (Spring-8 Angstrom Compact free electron Laser) in Harima, Japan produced its ﬁrst beams in 2011. Others are being built: the European source XFEL in Hamburg, Germany and SwissFEL in Villigen, Switzerland, PAL (Pohang Accelerator Laboratory) in Korea.

4C.3. Neutrons Neutrons are particles with rest mass mn = 1.67 ×10−27 kg, with no electric charge but with a magnetic moment μn = −0.97 ×10−26 J T−1 with the minus sign indicating that the magnetic moment is in the direction opposite to the spin. Neutron beams are produced either from nuclear reactors, using ﬁssion, or from spallation sources in which high energy proton beams interact with a target, usually in a pulsed mode5 . Examples of research reactors are the multinational Institut Laue-Langevin (ILL), and Orphée at the Laboratoire Léon Brillouin in Saclay, near Paris. ISIS, in England, or the Spallation Neutron Source (SNS) in Oak Ridge, TN, USA, are spallation sources. In either case, the initial energy of the neutrons, in the MeV range, is much too high for structural investigations, and they have to be submitted to a decrease in their kinetic energy, a process called moderation. They have De Broglie wavelength in the right range, around 1 Å, if their kinetic energy Ec = p2 /2mn = h2 /2mn λ2 , where p is their momentum, is a few tens of meV. A diﬀerent way of expressing this condition is that the kinetic energy then corresponds to a thermal energy kB T where kB = 1.38 ×10−34 J K−1 is Boltzmann’s constant and T a temperature in the range around room temperature, i.e. 300 K. This description is meaningful because preparing neutron beams in the right range of energy is actually performed by letting the neutrons, which cannot be tailored by electric ﬁelds, collide with a moderator material, such as heavy water D2 O, at this temperature. They are usually called “thermal neutrons”, while neutrons with higher energy, obtained through moderation in a hot object, are “hot neutrons”, and those with lower energy are “cold” or “ultra-cold” neutrons. As in the case of synchrotron radiation, single-energy beams must be extracted through the use of monochromators. The intensity of neutron beams is smaller than that of X-ray beams from laboratory generators, and very much smaller than X-ray beams from synchrotron radiation. Furthermore, neutrons are only available at large facilities, which implies the same diﬃculties in access as for synchrotron radiations. This leads to their use being far less wide-spread than X-rays, and restricted to investigations where their special features are a bonus.

5. Recommended reading includes two courses by Roger Pynn: http://www.ncnr.nist.gov/summerschool/ss09/pdf/Lecture_1_Theory.pdf, and http://link.springer.com/book/10.1007/978-0-387-09416-8/page/1.

Chapter 4 – Relationship between space groups and point groups

79

4C.4. Electrons Electrons are particles with electric charge −e = −1.6 ×10−19 C, with rest mass me = 0.9 ×10−30 kg. Their magnetic moment, associated to the intrinsic angular momentum or spin, has a direction opposite to the spin. Its absolute value is 1 Bohr magneton (1μB ) = 0.93 ×10−23 J T−1 , much larger than the neutron’s but whose inﬂuence is hidden by the eﬀect of the charge. The relation between the kinetic energy eU , obtained through acceleration under voltage U , and the De Broglie wavelength of an electron6 is: λ= √

1 h . 2m0 eU 1 + eU 2 2m0 c

Electrons with wavelength in the range of 10−10 m are unable to penetrate materials, and they can provide information from a very thin region near the surface (Low Energy Electron Diﬀraction, LEED). Higher energy electrons (100 keV or more) are used for the investigation of thin ﬁlms (less than 1 micrometer) in electron microscopes. These allow switching between the imaging and diﬀraction modes, i.e. between the observation of direct and reciprocal space, at the press of a button. They are complementary to X-rays for some crystal structure investigations, in particular for materials where only tiny crystalline regions can be obtained.

Further reading J. Als-Nielsen, D. McMorrow, Elements of Modern X-ray Physics, 2nd edn. (Wiley, 2011) R. Scherm, B. Fåk, Neutrons, in Neutron and Synchrotron Radiation for Condensed Matter Studies, vol. 1: Theory, Instruments and Methods, ed. by J. Baruchel et al. (Les Editions de Physique and Springer-Verlag, 1993) R. Pynn, Introduction to Neutron Scattering. A clear and comprehensive exposition is available on http://knocknick.ﬁles.wordpress.com/2008/04/neutronsa-primer-by-rogen-pynn.pdf. The “rogen” in the address is a misprint for “roger”; in case it gets corrected at some point, the revised address could be tried in case of diﬃculty.

6. The general expression for the De Broglie wavelength of a particle is the relativis tic expression λ = h/p = hc/pc, with pc = E 2 − m20 c4 . It is well introduced in http://hyperphysics.phy-astr.gsu.edu/hbase/quantum/debrog2.html#c2. The limiting cases for zero rest mass (ultrarelativistic case, e.g. photons) and for kinetic energy small with respect to the rest mass energy (non-relativistic case, e.g. thermal neutrons) are easily retrieved.

80

Symmetry and Physical Properties of Crystals

Appendix 4A. General features of groups Deﬁnition A group is a set G of elements g1 , g2 . . . featuring an internal composition law, here denoted as •, so that f = gi • gk , and f is an element of G. This composition law is associative: gi • (gk • gl ) = (gi • gk ) • gl , so that the parentheses can be omitted in this product has a neutral element e such that gi • e = e • gi = gi is such that each element gi has an inverse g−1 such that gi • g−1 = i i −1 gi • gi = e. In what follows, we will omit the sign •. Order of the group If G is an inﬁnite set of elements, we say that the group is inﬁnite. Otherwise, we say that it is ﬁnite, and the order of the group is the number of its elements. Generating elements These are elements of the group such that all the elements of the group can be obtained as products of powers of these elements with one another or with their inverses. Rearrangement theorem The multiplication table of group is a dual-entry table (Sect. 2.3). All elements of the group appear on each row and each column of the table, and no element appears twice on a given row or column. This means that if x = y, then xz = yz. Proof: if xz = yz, then xzz −1 = yzz −1 and x = y, which is contrary to the assumption. Note that each row or column of the multiplication table contains all the elements of the group, but ordered diﬀerently from the preceding row or column. This is why this is referred as rearrangement theorem. Subgroup A subgroup H is a part of the elements of group G that forms a group with the same composition law as group G itself. We will show that, if group G is ﬁnite, the order nG of G is a multiple of the order, nH , of H. The ratio i = nG /nH is called the subgroup index. Invariant subgroup A subgroup H (with elements denoted as hi ) of G is invariant if, for any element s of G and hi of H, we have s−1 hi s = hj or hi s = shj .

Chapter 4 – Relationship between space groups and point groups

81

Partition of a group G modulo a subgroup H This is a classiﬁcation of elements of group G. We start out by considering the elements of H and withdrawing them from G. Then there remains in G at least one element x. We form all the products xhi . This set is denoted as xH and we remove it. We show that xH is disjoint from H. Assume in contrast that xhi = hj . Right-multiplying both sides of this equation by h−1 i , we obtain , which is an element of H since H is a group. But this is contrary x = hj h−1 i to the starting assumption (x is not in H). If there still remains in G an element y, we form the subset yH, we withdraw it from what remains of G, and so forth till there is nothing left. We can write G = H + xH + yH + . . . We show that xH and yH are disjoint by noting that, if we had yhi = xhj , then y = xhj h−1 i = xhk and this is contrary to the assumption (y is not in xH). Each subset xH or yH is called a coset. Since each coset of this partition has the same number of elements as H, we deduce that, if H and G are ﬁnite, the order of G is a multiple of the order of H. The above partition was performed by left-multiplying the elements of H with x, y, etc. It could have been made by choosing right-multiplication. Both partitions have no reason to be identical. In contrast, they are identical if H is invariant, because then xhi = hj x and in this case the set xH is identical to the set Hx. Quotient group Consider the partition of G by an invariant subgroup H. We show that the cosets xH, yH, etc. form a group which is called the quotient group of G by H and is denoted by G/H. The product of two elements xH and yH of this group is deﬁned as the set of elements obtained through the product of one of the elements of xH by one of the elements yH, i.e. xhi (yhk ) = x(hi y)hk = x(yhp )hk

because of the associativity in G, since H is invariant,

= xy(hp hk ) through associativity in G, = xyhm

because H is a group.

We deduce that the product of xH by yH is xyH, i.e. (xH)(yH) = (xy)H. The product xy cannot be within H since x and y are outside H, and thus xy = z with z ∈ / H and z = x or y; otherwise x or y would be the neutral element of G which is also the neutral element of H, and thus within H. Thus (xH)(yH) = zH. Associativity is obvious since associativity applies within G. The neutral element is H, since hi (y hn ) = hi (hp y) = (hi hp )y = hv y = yhw and thus H(yH) = yH. The inverse of xH is x−1 H since xhi x−1 hn = xx−1 hp hn = hq .

82

Symmetry and Physical Properties of Crystals

Abstract groups A group can be deﬁned by the name of its elements and their multiplication table without reference to concrete examples. It is then referred to as an abstract group. Here are two examples: 1.

Cyclic groups They are groups denoted as Cn which have n elements such that, if one is denoted as A, the others are A2 , A3 ,. . . ,An = E where E is the neutral element. For example, group C3 consists of an element A, of element A2 and of the neutral element E = A3 . Its multiplication table is given below A

A2

E

A

A2

E

A

A2

E

A

A2

E

A

A2

E

As we will see, a concrete realization of this group is the group of rotations by 2π/3 around an axis, i.e. in terms of point groups, group 3. 2.

Dihedral groups A dihedral group is deﬁned using two generating elements A and B which satisfy relations B2 = E, An = E and BA = An−1 B. It includes 2n elements and is denoted as Dn . We will see that a concrete realization of group D3 is for example point group 32, for which A is the rotation by 2π/3 about a given axis and B is the rotation by π around an axis perpendicular to the above.

Chapter 5

Point groups The point groups are enumerated in a rigorous way. On ﬁrst reading, the reader can be content with their geometrical representation using the stereographic projection (Sect. 5.2) and with their denomination and classiﬁcation by crystal system (Sect. 5.6).

5.1. Introduction The point group of a crystal governs the symmetry of its physical properties. We recall that the point group consists of the symmetry operations of the crystal with all the translations removed. All the symmetry elements are assumed to go through a given point O. Further, we saw (Sect. 2.1) that the symmetry elements which do not contain a translation are either rotations or rotoinversions. The rotations are operations which conserve the handedness of a trihedron (proper operations), while the rotoinversions, which do not conserve the handedness of a trihedron, are said to be improper operations. We showed (Sect. 4.3) that the symmetry operations of the point group form a subset of the point group of its crystal lattice. This property also results from Curie’s principle (Sect. 3.3.5) because the crystal lattice is a property of the crystal and therefore it must be at least as symmetric as the crystal. This is a basic result, because it restricts the number of proper crystallographic point groups (groups which contain only proper operations, i.e. rotations). Since the only symmetry axes which a crystal lattice can feature are the 2-, 3-, 4- or 6-fold axes, the proper symmetry operations of crystals are the symmetry operations associated to 2-, 3-, 4- or 6-fold axes. We will ﬁrst enumerate the proper crystallographic point groups (Sect. 5.4), after showing that the improper groups always contain a proper subgroup with order half their own (Sect. 5.3). This property will be used in Section 5.5 to enumerate the improper groups starting from the proper groups. Sections 5.3, 5.4 and 5.5 show how to logically enumerate the 32 crystallographic point groups. In a ﬁrst approach, the reader may accept that there are 32 point groups, and get acquainted with them straight away in Section 5.6, where they are grouped into crystal systems. In contrast, reading

© Springer Science+Business Media Dordrecht 2014 C. Malgrange et al., Symmetry and Physical Properties of Crystals, DOI 10.1007/978-94-017-8993-6_5

83

84

Symmetry and Physical Properties of Crystals

Section 5.2, which introduces the stereographic projection used to represent the point groups, is mandatory. The chapter closes with a short discussion of isotropy groups in Section 5.9. They are not crystal point groups, but they enter the investigation of the physical properties of crystalline materials.

5.2. Stereographic projection 5.2.1. Deﬁnition It is very useful to represent, for a given point group, the directions equivalent to a given general direction, i.e. the directions obtained from this direction by applying all the symmetry operations which make up this group. For a general direction, i.e. a direction which is not parallel to a symmetry axis (n-fold or n ¯ -fold axis), there is one direction for each symmetry operation, and therefore there are as many equivalent directions as there are symmetry operations in the group. A precise two-dimensional representation of these equivalent directions requires a projection of three-dimensional space onto the plane of the drawing. The projection used by crystallographers is the stereographic projection, deﬁned below. Let O be the intersection of the various symmetry elements (rotation or rotoinversion axes).1 A given general direction is represented by a half-line Ov starting from this point O. This half-line intersects a sphere with center O and with any radius R at a point P which characterizes the direction (Fig. 5.1a). Representing the half-lines is tantamount to projecting the points P of the sphere onto a plane. We choose a projection plane Π which goes through the center of the sphere. This plane Π intersects the sphere along a circle C. We draw the diameter NS perpendicular to plane Π; N is the north pole, S the south pole, Π is the equatorial plane and circle C the equatorial circle. Let Ov be a direction in the northern hemisphere. Consider the meridian plane deﬁned by axis NS and point P (Fig. 5.1b). The line SP of this plane intersects the equatorial projection plane Π at n, which is the required projection. The triangles NPS and nOS are similar, and SN/Sn = SP/SO. We obtain Sn . SP = SN . SO = 2R2 . Point n is therefore deduced from P through an inversion with pole S and power 2R2 . Recall the deﬁnition of the inversion transformation. An inversion with pole O and power k transforms a general point M into an image point M such that O, M and M are aligned and OM . OM = k. Inversion conserves angles and transforms a circle that does not go through pole O into a circle.

1. For rotoinversion axes, this is also the position of the center of symmetry used for the rotoinversion operations.

Chapter 5 – Point groups N

N

v

v P

P

A

O

A

n

C

85

O

B

B

x

n

n'

P' v'

S

S

(a)

(b)

N A A

O

m

B

n'

O

n 9

m B

P' v' S

(c)

x

(d)

Figure 5.1: Principle of the stereographic projection. (a) The general direction Ov intersects the sphere at P. (b) n and n are respectively the transforms of P and P in inversions with pole S, the south pole. (c) m is the transform of P through inversion with pole N, the north pole. (d) n and m are the stereographic projections of the directions Ov and Ov respectively. Point P is deﬁned by its spherical coordinates R, θ and ϕ (axis Ox is a general direction in plane Π), and its projection n by its polar coordinates ρ and ϕ in plane Π. The length ρ = On is easily calculated when we notice that (SP, SN) = α = θ/2. Hence On = R tan α = R tan(θ/2). It is important to note that the azimuthal coordinate ϕ is conserved by the stereographic projection. Now consider a direction Ov in the southern hemisphere, and, in order not to clutter the text with more ﬁgures than necessary, assume it is in the same meridian plane as the above direction Ov (Fig. 5.1b). It intersects the sphere at P . Its projection n , deﬁned as above, is outside the equatorial disk. The closer P comes to the south pole, the further n moves away from O. This would lead, in order to represent all the directions of space, to using an inﬁnite surface! To avoid this diﬃculty, we use, for the directions of the southern hemisphere, an inversion with pole N, and with the same power 2R2 (Fig. 5.1c). The projection m of direction Ov is now located inside the equatorial disk. The stereographic projection is thus deﬁned as an inversion with pole S (the south pole) for the directions located in the northern hemisphere, and an inversion with pole N (the north pole) for the directions in the southern hemisphere. Thus the same

86

Symmetry and Physical Properties of Crystals

point will be the projection of two directions, symmetric to each other with respect to the projection plane Π. To distinguish these projections, one uses two diﬀerent symbols, for example crosses for the projections of the directions in the northern hemisphere, and circles for those of the southern hemisphere (Fig. 5.1d). The equatorial disk thus contains the stereographic projections of all the directions of space.

5.2.2. Examples Consider the point group 3, i.e. the group whose elements are the rotations by 2π/3, 4π/3 and 2π (identity) around a given 3-fold axis denoted as A3 . We choose as projection plane for the equivalent directions a plane perpendicular to this axis A3 . The projection of the axis itself is point O, the common projection of the directions ON and OS. Consider a general direction Ov, the stereographic projection of which is n, with polar coordinates (ρ = On, ϕ) (Fig. 5.1a). Rotation around axis NS causes rotation of the meridian halfplane containing Ov and conserves angle θ, hence ρ. The projections of the three directions equivalent to Ov through the three symmetry operations of the group are n (ρ, ϕ + 2π/3) for the rotation by 2π/3, n (ρ, ϕ + 4π/3) for the rotation by 4π/3 and n itself for the rotation by 2π or identity (Fig. 5.2). We understand, using this simple example, that the number of directions equivalent to a given general direction is equal to the number of elements in the symmetry group, or order of the group. Of course this is no more true if the direction is special, as would be the direction of the axis itself, which is invariant through the symmetry operations, and the stereographic projection of which is O. n’

O

n

n”

Figure 5.2: Stereographic projection of a general direction (projection at n) and its equivalent directions through the symmetry operations associated to an axis A3 The point symmetry elements featured by a crystal with a given crystal group appear directly on the stereographic projection of the directions equivalent to a general direction through the symmetry operations of the group. In what follows, we will simplify our description by simply referring to the “stereographic projection of the equivalent directions”, the remainder of the sentence being implied. A few examples are illustrated on Figure 5.3. The derivation of the results is either evident, or given in Appendix 5A.1. The thick lines represent the stereographic projections of planes, while the thin lines are just aids for the drawing.

Chapter 5 – Point groups

87 B

O

7

B

O A

A

(a)

B

O

O A

(b)

(c)

(d)

Figure 5.3: Stereographic projections of various symmetry elements and of the directions equivalent through the symmetry operations to which they are associated: (a) mirror in the projection plane; (b) mirror perpendicular to the projection plane; (c) 2-fold axis in the projection plane; (d) general mirror intersecting the projection plane along AB Mirror parallel to the projection plane: it coincides with plane Π. Its stereographic projection is the equatorial circle. Two directions which are equivalent through the mirror operation project on the same point with diﬀerent symbols, since one of the directions is in the northern hemisphere and the other in the southern hemisphere (Fig. 5.3a and Appendix 5A.1.2). Mirror perpendicular to the projection plane: it goes through axis NS and its projection is the line where the mirror intersects the plane of projection, i.e. AB on Figure 5.3b. The equivalent directions are in the same hemisphere and their stereographic projections are two points with the same nature (cross or circle), symmetric with respect to the line representing the projection of the mirror (Appendix 5A.1.3). n-fold axis, noted An or n, perpendicular to the projection plane: the projection of the axis consists in two points coinciding with the center of the equatorial circle. It is represented by a single symbol, characteristic of its order n. The conventional symbols are given in Table 5.1. The equivalent directions, all located in the same hemisphere, project on points which deduce from one another through rotations by 2π/n around the axis, and which are represented by the same sign (Fig. 5.4). Table 5.1: Graphical representation of the symmetry axes Axis type 2

Graphical representation

Axis type _ 1

4

_ 3 _ 4

6

_ 6

3

Graphical representation

88

Symmetry and Physical Properties of Crystals

2

3

4

6

Figure 5.4: Stereographic projections of directions equivalent through the symmetry operations associated to 2-, 3-, 4- and 6-fold axes 2-fold axis parallel to the projection plane: the projection of the axis consists in two points A and B, the intersections of the axis and the equatorial circle (Fig. 5.3c). These points are displayed using the symbol characteristic of the 2-fold axes. The equivalent directions are in diﬀerent hemispheres, and their projections are symmetric with respect to line AB (Appendix 5A.1.4). Mirror with general orientation: such a mirror intersects the projection plane along a line AB. The stereographic projection of the mirror consists of two circular arcs going through A and B and symmetric with respect to AB (Fig. 5.3d and Appendix 5A.2.1).

5.2.3. Application to rotoinversion axes or n ¯ -fold axes The deﬁnition of n ¯ -fold axes was given in Section 2.2.2, but their properties can become clearer using the new tool we now have. Figure 5.5 shows the stereographic projections of equivalent directions for these various rotoinversion axes. The projection plane is perpendicular to the n ¯ axis, and goes through the inversion center used for the rotoinversion.

7 7

7

7

– 1

– 2

– 3

– 4

– 6

Figure 5.5: Stereographic projections of directions equivalent through the symmetry operations associated to ¯1, ¯2, ¯3, ¯4 and ¯6-fold axes We note that: a ¯3-fold axis is equivalent to the set consisting of a 3-fold axis (coinciding with the ¯3-fold axis) and a center of symmetry;

Chapter 5 – Point groups

89

a ¯6-fold axis is equivalent to the set consisting of a 3-fold axis (coinciding with the ¯6-fold axis) and a mirror perpendicular to this axis and going through the inversion center used for the rotoinversion; a ¯4-fold axis has no equivalent. ¯ We retrieve the fact that a 1-fold axis is equivalent to a center of symmetry and a ¯2-fold axis to a mirror perpendicular to the axis and going through the center of symmetry used for the rotoinversion. We can note that the order of the n ¯ groups is equal to n, except for the group ¯3 for which the order is 6.

5.2.4. Family of equivalent directions We saw in Chapter 3 that a crystal row is noted [uvw] if the vector V joining two neighboring nodes on the row can be expressed as: V = ua + vb + wc, where a, b and c are the basis vectors of the crystal unit cell. Since the physical properties of a crystal are identical along two directions equivalent through the symmetry operations of its point group, it is often necessary to consider not only a direction parallel to a row [uvw], but the set of directions equivalent through the symmetry operations of the point group. The set of these equivalent directions is noted < uvw >. In the same way, the set of lattice planes equivalent to a lattice plane (hkl) through the symmetry operations of the point group is noted {hkl}. However, we must note that [uvw] represents a row of nodes and is not oriented. In the same way, (hkl) is a lattice plane and its normal is not oriented. When directions equivalent through the symmetry operations of the point group are considered, it is necessary, for the non-centrosymmetric groups, i.e. those which do not contain inversion, to orient the direction. For example, in a crystal with the cubic point group ¯43m, <111> is diﬀerent from < ¯1¯1¯1 > and, in the same way, {111} is diﬀerent from {¯1¯1¯1} (Exercise 5.6). The name given to {hkl} is a “crystal form”. The reason is that the growth rate of a crystal is the same for all the equivalent (hkl) planes. If the external shape or form of the crystal (its “habit”) features an (hkl) orientation, then the whole set of faces equivalent to (hkl) are encountered, whence the name “crystal form” for {hkl} (assuming of course that special external interactions, which could hamper the growth of some faces, are not present).

5.3. Improper groups 5.3.1. Preliminary remark For a given group, we will note Si its proper symmetry operations (rotations) and Sj its improper symmetry operations (rotoinversions). We recall that the

90

Symmetry and Physical Properties of Crystals

product of two proper operations or of two improper operations is a proper operation, and that the product of a proper operation and an improper operation is an improper operation. By deﬁnition, a proper group contains only proper operations, and an improper group contains one or several improper operations. However an improper group contains at least one proper operation: the neutral element. We can therefore write any group G as the sum of a set of proper elements, among which the neutral element E or identity, and of a set of improper elements which is an empty set when G is a proper group: G = {E, S1 , S2 , . . .} + {S1 , S2 , . . . }.

5.3.2. Properties of improper groups The proper elements of an improper group form an invariant subgroup with order half that of the improper group. 1.

They form a group because the product of two proper elements is a proper element, the neutral element is a proper element and the inverse of a proper element is a proper element.

2.

This subgroup is invariant. This requires showing that, for any element s of the group, s−1 Si s = Sj (Appendix 4A). This is evident if s is a proper element. If s is improper and noted as Sk , its inverse Sj is also improper, and we obtain a proper element for the product Sk Si Sj .

3.

This subgroup is of order half that of the group. We will show that an improper group contains as many proper elements as improper elements.

Let np be the number of proper elements and ni the number of improper elements of the group. Consider a given improper element Sm , and multiply it successively by i)

all the np proper elements: Sm Sk = Sl . We obtain np improper elements, all diﬀerent from one another (see the rearrangement theorem derived in Appendix 4A). Therefore np ≤ ni .

ii) all the ni improper elements: Sm Sk = Sl . We obtain ni diﬀerent proper elements, and ni ≤ np . The conclusions of (i) and (ii) imply that ni = np . We deduce from (1), (2) and (3) that an improper group always contains a proper subgroup with order half its own and invariant.2 2. It can be shown that a subgroup of order half is always invariant. Therefore we could have just shown that the subgroup is of order half.

Chapter 5 – Point groups

91

We now enumerate ﬁrst the proper groups, then the improper groups starting from the proper groups.

5.4. Enumeration of the proper point groups 5.4.1. Preamble We recall that the elements of a proper point group are rotations by 2π/n and their multiples around a given axis, with the condition (Sect. 3.3.2): n = 1, 2, 3, 4, or 6 (condition 1). The simplest groups are those which contain only the symmetry operations resulting from the presence of a single symmetry axis, an n-fold axis, often noted as An . They will be enumerated in Section 5.4.2. We then consider the groups which contain symmetry operations associated with the existence of two axes, An and An , where n and n satisfy condition 1. The combination of two of these operations, i.e. the product of a rotation by 2π/n (or one of its multiples) around axis An and a rotation by 2π/n (or one of its multiples) around axis An must also satisfy condition 1, i.e. be a rotation by 2π/n (or one of its multiples) around an axis, with n also fulﬁlling condition 1. This restriction on n leads to the following results: 1.

For a general value of n, n is equal to 2 and the angle between the two axes is equal to 90◦ . The corresponding groups are described in Section 5.4.3.

2.

For n = 2 or 4, n can also be equal to 3 and the angle ω between the 3-fold axis and the 2- or 4-fold axis is then such that cos2 ω = 1/3, i.e. the angle between a side and a major diagonal of a cube. The corresponding groups (cubic groups) are described in Section 5.4.4.

The approach used to derive these results is the following. Let ω be the angle between axes An and An and O their intersection point (Fig. 5.6). We choose a system of axes Oxyz such that axis Oz be parallel to axis An and axis Ox be perpendicular to the plane deﬁned by An and An . The matrix Sn representing the rotation around axis An is easily expressed in the axis system Oxyz. The matrix Sn representing the rotation around axis An is easily expressed in a system of axes Oxy z where Oz is parallel to An , and it is noted Sn . To obtain the matrix Sn for the rotation around An in the axis system Oxyz, we use the transition matrix R for passage from the referential Oxy z to the referential Oxyz. We know that Sn = R−1 Sn R. The product Sn Sn is a matrix for which the trace must be an integer in order to satisfy the condition n = 1, 2, 3, 4 or 6 (Sect. 3.3.2). The calculation is simple but tedious, and will not be presented here.

92

Symmetry and Physical Properties of Crystals An’ An z z’

O

y’ y

x

Figure 5.6: Systems of orthonormal axes used to obtain the product of a rotation around an axis An and a rotation around another axis An’ . Axis Ox is perpendicular to the plane containing An and An’ .

5.4.2. Groups containing only the symmetry operations associated to an axis An (cyclic groups) Note: for simplicity, the title of this section could be replaced by “groups featuring only an axis An ”, and this is what we will often do in what follows even though this formulation is not very accurate. The elements of the group are the symmetry operations associated to the symmetry element, for example the rotations by π/2, π, 3π/2 and 2π for a group “featuring an A4 axis”. There are ﬁve such groups, corresponding to n = 1, 2, 3, 4 and 6, and they are noted n in the Hermann-Mauguin notation which we use in this book. Group 1: no symmetry operation in this group, which contains only the identity element. Group 2: existence of an axis A2 . The symmetry operations are the rotation by π around this axis and the rotation by 2π, i.e. identity. Group 3: existence of an axis A3 . The symmetry operations are the rotations by 2π/3, 4π/3 and 2π (identity) around the axis. Group 4: existence of an axis A4 . The symmetry operations are the rotations by 2π/4 = π/2, π, 3π/2 and 2π (identity) around the axis. Group 6: existence of an axis A6 . The symmetry operations are the rotations by 2π/6 = π/3, 2π/3, π, 4π/3, 5π/3 around the axis, and identity. Figure 5.4 shows the stereographic projection of the equivalent directions for each of these groups. The projection plane is perpendicular to axis An . The number of equivalent directions, equal to the order of the group (Sect. 5.2.2), is equal to n. The corresponding abstract groups are the cyclic groups Cn (Appendix 4A).

5.4.3. Groups containing the symmetry operations associated to an axis An and to a perpendicular axis A2 , or dihedral groups An elementary geometrical argument shows that, if there exist a symmetry axis An and an axis A2 which is perpendicular to it and intersects it at point O,

Chapter 5 – Point groups

93

then there exist n axes A2 going through O, orthogonal to axis An , and with an angle π/n between them (Exercise 5.1). This can also be shown using the stereographic projection (Exercise 5.2). These groups are called n2 if n is odd (group 32) and n22 if n is even (groups 222, 422, 622). The second “2” in the latter cases may seem redundant. Its presence will be justiﬁed when we describe the space groups. The corresponding abstract groups are the dihedral groups Dn (Appendix 4A). Figure 5.7 shows, for each of these groups, the stereographic projection of the equivalent directions and of the symmetry elements.

222

32

422

622

Figure 5.7: Dihedral point groups. They feature one An axis and n 2-fold axes which are perpendicular to An .

5.4.4. Cubic proper groups These are groups for which the generating elements are the symmetry operations associated to a 2-fold (or 4-fold) axis and a 3-fold axis, with the angle between them equal to that between one side of a cube and a major diagonal of this cube. By working out the product of the various symmetry operations associated to the 2-fold (or 4-fold) axis and the 3-fold axis, it can be shown that there are then three 2-fold (or 4-fold) axes parallel to the three sides of a cube, and four 3-fold axes, parallel to the major diagonals of the cube (Exercise 5.3). The two groups thus deﬁned are called 23 and 432. The notation for the cubic groups consists of two or three symbols. The ﬁrst one concerns the symmetry axes parallel to the sides of the cube, the second one the 3-fold axes parallel to the major diagonals of the cube, and the third, if it exists, indicates the presence of axes parallel to the diagonals of the cube faces. We will see later that, in the cubic groups featuring mirrors, the same rule applies when considering the directions perpendicular to the mirrors. Thus the notation 23 indicates the presence of 2-fold axes parallel to the sides of a cube and of 3-fold axes parallel to the major diagonals of the cube. There is no third symbol because there are no symmetry axes parallel to the diagonals of the cube faces. The group 432 involves three 4-fold axes parallel to the sides of the cube, four 3-fold axes parallel to the cube diagonals, and six 2-fold axes parallel to the diagonals of the six cube faces. Figure 5.8 shows, for each of these groups, the stereographic projection of the equivalent directions and the symmetry elements.

94

Symmetry and Physical Properties of Crystals

23

432

Figure 5.8: Proper cubic groups

5.5. Enumeration of the improper point groups We saw that any improper group G contains a proper (and invariant) subgroup of order half. Let us note it as Gp . The group G can thus be decomposed into cosets starting from Gp : ¯ p = {S1 , S2 , . . . , Sp } + {AS ¯ 1 , AS ¯ 2 , . . . , AS ¯ p} G = Gp + AG ¯ is any improper element of G. If G contains inversion, a partition into where A ¯ these two cosets is evident since inversion itself can be chosen as the element A. This is discussed in the next section. We will see in Section 5.5.2 how to obtain those improper groups that do not contain inversion.

5.5.1. Improper groups containing inversion These are obtained by considering successively all the proper groups previously deﬁned, and adding to them one generating element, inversion I (and consequently all the elements that are the product of an element of Gp and of inversion): G = {Gp } + I{Gp }. The stereographic projection of the directions equivalent through the symmetry operations of the group is a good tool to determine all the symmetry operations of the groups G thus obtained. The ﬁrst, almost trivial, example, is that of group 1, the only element of which is identity, to which one adds inversion I. The group contains two elements, the neutral element or identity E, and inversion I. It is noted as ¯1, since a ¯1 axis is equivalent to a center of symmetry (Fig. 5.5). Groups deduced from the cyclic groups Consider the proper group 2 and the improper group to which it is associated by adding inversion. We draw the stereographic projection of the equivalent directions onto a plane perpendicular to the 2-fold axis (Fig. 5.9). Consider an initial direction, and suppose it is in the northern hemisphere. Its stereographic

Chapter 5 – Point groups

95

projection is a cross at point 1. The direction equivalent through a rotation by π around the axis has for its stereographic projection a cross at point 2. Let us add a center of symmetry. The projection of the direction equivalent to 1 through inversion is a circle (since it is a direction in the southern hemisphere) at point 3 coinciding with point 2, and that of the direction equivalent to 2 through inversion is a circle at point 4 coinciding with 1. We therefore immediately see there is a mirror perpendicular to the 2-fold axis.

17 37

4

2

Figure 5.9: Point group obtained by adding inversion to group 2 The group we are discussing has 4 elements, corresponding to the four stereographic projections: identity E associated to the projection 1 of the initial direction, rotation by π around the axis, which we note as A, associated with projection 2 (2 is the transform of 1 through A), inversion I associated to 3 (3 is the transform of 1 through I), and the mirror operation m perpendicular to the axis, associated to 4 (4 is the transform of 1 through m = IA). The generating elements of the group are A and I (the fourth element is then m = AI) or A and m (and the fourth element is I = Am). The notation for this group refers to the second choice. It is noted as 2/m, the position of m as the denominator to 2 meaning that the mirror is perpendicular to the 2-fold axis. Figure 5.10 shows the stereographic projections of the improper groups thus determined by adding inversion to the cyclic groups of Figure 5.4, and their denominations. They are noted 2/m, ¯3, 4/m and 6/m. We recall that the existence of a ¯3-fold axis is equivalent to the presence of a 3-fold axis and of a center of symmetry. 7 7 7

7 7

2 — m

7

7

7

– 1

7

7

– 3

4 — m

7

7

6 — m

Figure 5.10: Point groups obtained by adding inversion to groups 1, 2, 3, 4 and 6

96

Symmetry and Physical Properties of Crystals

Groups deduced from the dihedral groups Consider group 222 and the stereographic projection of the 4 directions equivalent through the symmetry operations of the group onto a plane perpendicular to one of the 2-fold axes (Fig. 5.11a). Let us add inversion to these symmetry operations. We obtain, on the stereographic projection, four further directions, the directions opposite to the above (Fig. 5.11b).

7 7

7 7

222

mmm

(a)

(b)

Figure 5.11: Group 222 and group mmm, deduced from 222 by adding inversion This projection reveals three mirrors perpendicular to the 2-fold axes, and mutually perpendicular. The group is noted mmm because the three mutually orthogonal mirrors can be chosen as generating elements. The presence of the 2-fold axes then results from the product of the mirror operations taken pairwise. In the same way, if inversion is added to group 422, we obtain a 4-fold axis, four mirrors going through the 4-fold axis and enclosing an angle of π/4 between each other, and a mirror perpendicular to the 4-fold axis. The generating elements of the group are the 4-fold axis, a mirror going through the axis, and a mirror perpendicular to the axis. Its denomination is 4 ⁄ m mm. As above, the m as the denominator of the fraction indicates that the mirror is perpendicular to the 4-fold axis. The ﬁnal m is redundant, but its presence is justiﬁed when space groups are considered (Chap. 7). Figure 5.12 shows the stereographic projections of the equivalent directions in the improper groups thus determined, and their denominations (¯3m, 4 ⁄ m mm, 6 ⁄ m mm). 77 7 7

7 7 77

– 3m

7

4 —mm m

7

7

7

7 7

7 7 7

7

7

7

6 —mm m

Figure 5.12: Groups obtained by adding inversion to the dihedral groups 32, 422 and 622. The white circles at the centers of the symbols for the 3-, 4- and 6-fold axes indicate the existence of a center of symmetry.

Chapter 5 – Point groups

97

Groups deduced from the proper cubic groups Adding inversion to group 23 gives group m¯3 (Fig. 5.13, to be compared with Fig. 5.8). The ﬁrst sign (m) indicates that there are mirrors perpendicular to the sides of the cube, and the second sign indicates that the axes parallel to the major diagonals are ¯3 axes. There is no third sign because there are no 2-fold axes parallel to the face diagonals, nor mirrors perpendicular to these diagonals. 7 7 7

7 77 77

7

7 7 7

– m3

7 7 7 7 7 7 77 7 7 7 7 7 7 7 77 7 7 7 7 7 7 7

– m3m

Figure 5.13: Groups obtained by adding inversion to the proper cubic groups Adding inversion to group 432 leads to group m¯3m which features all the symmetry elements of a cube. The reader will check that the symmetry elements of a cube all go through the center of the cube and are the following: a center of symmetry, three 4-fold axes parallel to the cube sides and the mirrors perpendicular to them, four 3-fold axes coinciding with the major diagonals of the cube, six 2-fold axes parallel to the face diagonals of the cube, and the six mirrors which are respectively perpendicular to them, called diagonal mirrors. The denomination of the group also states that there are three mirrors perpendicular to the sides of the cube (ﬁrst m), four 3-fold axes parallel to the major diagonals of the cube and an inversion center (¯3), and six mirrors perpendicular to the face diagonals of the cube (m in third position). The 2-fold axes result from the combination of two orthogonal mirrors and lie at their intersection. The 4-fold axes result from the joint presence of mirrors parallel to the cube faces and of diagonal mirrors.

5.5.2. Improper groups which do not feature inversion We saw in Section 5.3.2 that any improper group G contains a proper invariant subgroup with order half. Let us denote it as Gp . Group G can therefore be split into two cosets starting from Gp : ¯ p = {S1 , S2 , . . ., Sp } + {AS ¯ 1 , AS ¯ 2 , . . ., AS ¯ p} G = Gp + AG ¯ is an improper element which we assume not to be inversion. Consider where A ¯ obtained by multiplying A ¯ and inversion I. This the proper element A = IA may look arbitrary, but we will soon see why it is of interest. Let us show, through a reduction toward the absurd, that A is not part of G or, more precisely, of Gp , since A is a proper element. If A belonged to Gp , then its

98

Symmetry and Physical Properties of Crystals

¯ which belongs to G, inverse A−1 would also be in Gp , and its product with A, −1 −1 −1 ¯ ¯ i.e. A A would be part of G. But A A = IA A = I and, by assumption, I is not in G. Therefore A is not an element of Gp . Consider the set G = Gp + AGp = {S1 , S2 , . . ., Sp } + {AS1 , AS2 , . . ., ASp }. The elements ASk do not belong to Gp . To show this, assume ASk is part −1 −1 of Gp . Since S−1 k is in Gp , the product (ASk )Sk = A(Sk Sk ) = A would also be in Gp , which is contrary to the above result. All the ASk are distinct, since if ASk = ASl , then left-multiplying with A−1 would yield Sk = Sl , which is contrary to the assumption. We now show that G and G are isomorphous, with the following correspondence: the elements of Gp correspond with one ¯ p is associated to ASp . Compare the multiplication tables of another, and AS G and G (Fig. 5.14), which we divided into four quadrants. The top left quad¯ k) = ¯ j )(AS rants are identical. So are the bottom right quadrants, since (AS (IASj )(IASk ) = (ASj )(ASk ) because of the commutativity of I with all the elements and because I2 = E. The top right quadrant contains, for G , the ¯ k ) = Sj (IASk ) = ISj (ASk ). products Sj (ASk ) and for G, the products Sj (AS The bottom left quadrants show for G the products (ASj )Sk and for G the ¯ j )Sk = (IASj )Sk = I(ASj )Sk . There is thus a one-to-one correproducts (AS spondence between the products in G and G. S1 S2

Sk

Sp AS1

ASk ASp

S1 S2 Sj

SjSk

Sj(ASk)

Sp AS1 AS2 ASj

S1 S2

Sk

– Sp AS1

– – ASk ASp

S1 S2 Sj

SjSk

ISj(ASk)

IASjSk

ASjASk

– Sp AS1 – AS1 ASjSk

ASjASk

– ASj – ASp

ASp

G’

G

Figure 5.14: Multiplication table of the isomorphous groups G and G The elements of the set G thus form a proper group of order 2p, isomorphous to G. To each group G2p containing a proper subgroup with order half there will correspond an improper group G as searched for. To obtain G starting from G2p and its subgroup Gp , we proceed in the following way: we separate in G2p the subgroup Gp and its complementary subgroup K, consisting of the operations K1 , K2 , . . . , Kp equivalent to the operations ASi : G2p = Gp + {Ki }.

Chapter 5 – Point groups

99

¯ i required to obtain G are the operations (IA)Si = I(ASi ) = The operations AS IKi . The required group G is: G = Gp + {IKj }. We start with the simplest example: that of group 2 (consisting of identity E and of the rotation A by π around the axis, i.e. {E, A}). This has as its subgroup with order half the group 1, which has as its sole element E. G = E+A and G = E+IA = {E, m} where m = IA is the symmetry operation with respect to a plane perpendicular to the 2-fold axis. This 2-fold axis was used as an intermediate device in the reasoning, but it is not a symmetry element of the group we are investigating. The improper group we are searching for has for its symmetry elements a mirror, and this group is denoted as m. In more complicated cases, the deﬁnition of G starting from G is made much easier by using the projection of the directions equivalent through the elements of G2p and of Gp . We take as an example group 422 and its subgroup with order half, 222. Figure 5.15a is the stereographic projection of the directions equivalent through the symmetry operations of group 422 (G2p ). We choose an initial projection direction, and denote it as 1. Figure 5.15b shows the directions equivalent to 1 through the symmetry operations of group 222 (Gp ). Figure 5.15c shows the equivalent directions for the required group G. The additional directions 5 , 6 , 7 , 8 are the reverse of directions 5, 6, 7 and 8, the complementary of directions 1, 2, 3 and 4 in obtaining 422 starting from 222. We see, on the projection of Figure 5.15c, that this group contains a ¯4-fold axis, two 2-fold axes perpendicular to this axis ¯4, and two mirrors parallel to axis ¯4 and enclosing angles of 45◦ to the 2-fold axes. This group is noted as ¯42m.

5 6 4 3

8’ 7’ 1 2

4 3

1 2

8 7

4 3

1 2 6’ 5’

422

222

– 42m

(a)

(b)

(c)

Figure 5.15: Construction of group ¯42m starting from group 422 (a) and its subgroup with order half, 222 (b) Figure 5.16 shows the stereographic projection of the equivalent directions in these various improper groups that do not contain inversion. We note that 1.

Any group 2n (abstract group C2n ) admits group n (abstract group Cn ) as a subgroup with order half (2→1), (4→2), (6→3) and these associations lead to groups m, ¯4 and ¯6 respectively (Fig. 5.16a).

2.

Groups n22 admit groups n as subgroups of order half, with the associations (222 → 2), (32 → 3), (422 → 4), (622 → 6), which lead to the

100

Symmetry and Physical Properties of Crystals

7 7

7

7

– 4

m

– 6

(a)

mm2

3m

4mm

6mm

(b) 7

7

7

7

7

– 42m

7

– 62m

(c)

– 43m

(d)

Figure 5.16: Point groups obtained from: (a) groups (2n) and their subgroups n; (b) groups n22 and their subgroups n; (c) groups 2p22 and their subgroups p22; (d) group 432 and its subgroup 23 groups mm2, 3m, 4mm and 6mm respectively, called pyramidal groups because they have the symmetry of regular pyramids with an n-fold axis and mirrors going through the axis (Fig. 5.16b). 3.

Groups n22 with n even, i.e. n = 2p, also admit the subgroups with half order p22, with the associations (422→222) and (622→32), which lead to groups ¯42m and ¯62m respectively (Fig. 5.16c).

4.

The cubic group 432 admits group 23 as a subgroup with order half, which leads to the group ¯43m (Fig. 5.16d). This is the symmetry group of a regular tetrahedron.

We thus deﬁned the 32 crystallographic point groups, which are 11 proper groups, 11 improper groups containing inversion, 10 improper groups that do not contain inversion.

Chapter 5 – Point groups

101

5.6. Classiﬁcation of the point groups The set of crystals having a given point group form a crystal class. All classes with the same lattice symmetry form a crystal system. Figures 5.17a and b show the classiﬁcation of point groups (hence of crystal classes) by crystal system. This classiﬁcation will be fully justiﬁed in Chapter 6. The qualitative presentation made here is an easy approach, suﬃcient on ﬁrst reading. We saw that there are seven crystal systems, deﬁned on the basis of the symmetry of the crystal lattice. We also saw that the crystal lattice is at least as symmetric as the crystal or, to put it diﬀerently, that the point group of the crystal is a subgroup of the point group of the crystal lattice or the group itself (Sect. 4.3). Simple examples of crystal point groups which are subgroups of the point group of the crystal lattice are the 21 point groups which do not contain inversion, while the point groups of all crystal lattices do contain inversion. We thus consider the seven point groups that have the symmetry of the seven crystal systems. Each of these groups is called a holohedral group. Each holohedral group is taken as the head of a row on which we arrange its respective subgroups. It is placed at the right-hand end of the row. On a given row, the number of elements of each group (the order of the group) grows from left to right, ending with the holohedral point group, the group of the crystal lattice. Figures 5.17 show, for all groups, the stereographic projection of their symmetry elements (Fig. 5.17a) and the directions equivalent to a given starting direction (Fig. 5.17b). The projection plane is perpendicular to the axis with the highest symmetry, except for groups 23 and m¯3, where the projection is performed, as for all cubic groups, on a plane perpendicular to one side of the cube. The starting direction is the same for all groups, so that the subgroups of the groups show up easily. Consider for example the crystals with an orthorhombic lattice. An orthorhombic lattice (unit cell in the shape of a rectangle parallelepiped) has for its symmetry elements 2-fold axes parallel to the sides of the parallelepiped, mirrors perpendicular to these axes, and a center of symmetry. The corresponding point group is group mmm (the third group starting from the left on the third row). The notation indicates the existence of three mutually orthogonal mirrors, the symmetry operations of which are the generating elements of the group. We showed the existence of crystal point groups 222 (three mutually orthogonal 2-fold axes) and mm2 (two mutually orthogonal mirrors, leading to the presence of a 2-fold axis at their intersection), which are subgroups of group mmm. It follows that a crystal with orthorhombic lattice can have for its point group 222, mm2 or mmm.

102

Symmetry and Physical Properties of Crystals

Triclinic

Bravais modes

P _ 1 - Ci P C (A) 2 - C2

222 - D2

m - Cs

mm2 - C2v

2/m - C2h P I F A (B) (C)

mmm - D2h

P I 4 - C4

_ 4 - S4

4/m - C4h

422 - D4

4mm - C4v

_ 42m - D2d 4/mmm - D4v

R P 3 - C3

_ 3 - C3i

6 - C6

_ 6 - C3h

Hexagonal

Rhombohedral (trigonal)

Tetragonal (quadratic)

Orthorhombic

Monoclinic

1 - C1

32 - D3

3m - C3v

_ 3m - D3d

P 622 - D6

6mm - C6v

Cubic

6/m - C6h

_ 62m - D3h 6/mmm - D6h

23 - T

_ m 3 - Th

432 - O

_ 43m - Td

_ m 3m - Oh

Figure 5.17a: The 32 crystallographic point groups arranged by crystal system: stereographic projection of the symmetry elements. The rightmost column indicates the Bravais modes consistent with each of the systems.

P I F

Chapter 5 – Point groups

103

Triclinic

Bravais modes

P

P C (A) 2

222

m

mm2

2/m P I F A (B) (C)

mmm

P I 4

_ 4

4/m

422

4mm

_ 42m

4/mmm

R P 3

Hexagonal

Rhombohedral (trigonal)

Tetragonal (quadratic)

Orthorhombic

Monoclinic

1

_ 1

_ 3

32

3m

_ 3m

P _ 6

6/m

622

6mm

Cubic

6

23

_ m3

432

_ 43m

_ m3m

_ 62m

6/mmm P I F

Figure 5.17b: The 32 crystallographic point groups arranged by crystal system: stereographic projection of the equivalent directions. The rightmost column indicates the Bravais modes consistent with each of the systems.

104

Symmetry and Physical Properties of Crystals

The arrangement of entries on the four ﬁrst rows is such that the crystal lattices are ranked in order of growing symmetry (triclinic, monoclinic, orthorhombic, tetragonal), easy to identify since the point group of a crystal lattice is a subgroup of the point group of the crystal lattice on the next row. Group ¯1 of the triclinic lattice is a subgroup of group 2/m of the monoclinic lattice, which itself is a subgroup of group mmm (orthorhombic lattice), while the latter is a subgroup of 4 ⁄ m mm (tetragonal lattice). We note that, to determine the row corresponding to a given point group, we look for the holohedral group with the lowest symmetry of which it is a subgroup: for example point group mm2 is a subgroup of the holohedral group mmm of the orthorhombic lattice. It is also a subgroup of point group 4 ⁄ m mm of the tetragonal lattice, but a crystal with point group mm2 has an orthorhombic, not a tetragonal, crystal lattice. It may occur, under speciﬁc temperature or pressure conditions, that a crystal with point group mm2 happens to have two lattice parameters equal, for example a = b. Such a crystal is then accidentally tetragonal. The rhombohedral and hexagonal lattices appear on the following rows. The point group of the rhombohedral lattice is a subgroup of that of the hexagonal lattice. We make an important note: we will show in Chapter 6 that the crystals with point group 3, ¯3, 32, 3m and ¯3m, all shown on the 5th row, can have either a rhombohedral crystal lattice (noted R) or a hexagonal crystal lattice (noted P). This is indicated by the two arrows pointing from this row to the rhombohedral and hexagonal lattices, as well as by the P associated to R in the column showing the Bravais modes. The cubic groups are shown on the last row. If the point group of the crystal is a subgroup of the holohedral group, the group is said to be merohedral. The table below shows the type of merohedry as a function of the ratio between the order of the holohedral group nH , viz. the order of the symmetry group of the crystal lattice, and the order of the merohedral group nM of the crystal. nH /nM

Designation of the group

1

holohedral

2

hemihedral

4

tetartohedral

8

ogdohedral

We recall the rules, already stated in Sections 5.4.2 to 5.4.4, of the HermannMauguin notation. A mirror parallel to an n-fold (or n ¯ -fold) axis is noted through an m next to the n (or n ¯ ), and a mirror perpendicular to an n-fold axis by an m as a denominator. For example group 3m involves a 3-fold axis

Chapter 5 – Point groups

105

and three mirrors parallel to this 3-fold axis. Group 4/m has a 4-fold axis and a mirror perpendicular to it. For the cubic groups, the ﬁrst symbol shows the order of the axes parallel to the cube axes (2 or 4) or the existence of mirrors perpendicular to these axes (m). The second symbol shows the existence of 3-fold axes parallel to the major diagonals of the cube, or ¯3 if there is also an inversion center. The third symbol, if it exists, shows the existence of 2-fold axes parallel to the diagonals of the cube faces or of mirrors perpendicular to these directions. Figure 5.17a also shows, next to this nomenclature which is the usual one for crystallographers, the Schönﬂies notation, frequently used in group theory, and summarized below: For all groups except for the cubic groups and groups ¯4 and m: ﬁnd the axis with the highest order, call it n, and assume it is vertical, associate to this group its cyclic (Cn ) or dihedral (Dn ) subgroup with the highest order, and start the notation with Cn or Dn respectively. This notation is complemented, if necessary, with a subscript i if there is also a center of inversion one of the following subcripts if there are mirrors: h if the mirror is horizontal, v if it is vertical and there is no horizontal 2-fold axis, or if there is a horizontal 2-fold axis in the plane of the mirror, d if the mirrors are vertical with 2-fold axes in the bisecting planes of the mirrors. Example: group 4mm, with subgroup C4 , has a vertical mirror as an extra generating element. It is noted C4v . The other notations are the following: notation Sn refers to the presence of a rotoinversion axis n ¯ , but it is used only for group S4 (¯4), because group ¯3 ¯ is noted as C3i (a 3-fold axis being equivalent to a 3-fold axis and a center of symmetry), and group ¯6 is noted C3h (a ¯ 6-fold axis being equivalent to a 3-fold axis and a mirror perpendicular to it). The notation Cs indicates group m (the s is from the German word Spiegel = mirror). The notations T (tetrahedron) and O (octahedron) are used for the cubic groups. T is the group of the rotations of the tetrahedron (group 23). It is easy to check, with the help of Figure 5.17b, that adding a horizontal mirror to group 23 yields group m¯3, therefore noted Th , while adding a mirror in the diagonal planes gives group ¯43m, noted Td . Group O is the group of the rotations of the cube (group 432), which becomes Oh (m¯3m) if a horizontal mirror is added.

106

Symmetry and Physical Properties of Crystals

5.7. Laue classes The investigation of X-ray diﬀraction by crystals shows that the intensity of the beams diﬀracted by a given crystal is the same whether the reﬂection3 occurs oﬀ one side or the other of the lattice planes. This result, known as Friedel’s law, only breaks down when the wavelength of the radiation is very near an absorption edge, i.e. when the energy of an X-ray photon is equal or nearly equal to that of an electronic energy level of one of the atoms in the crystal. Away from the absorption edges, diﬀraction thus introduces a center of symmetry even if the crystal structure has none. This is why the 32 symmetry groups are arranged into 11 sets such that the eﬀects of the crystal symmetry on diﬀraction are the same within each set. Each of the 11 centrosymmetric crystallographic groups deﬁnes one of these sets, called Laue classes. For any of the 21 remaining groups, just multiplying the group with (E, I) produces the centrosymmetric group which deﬁnes the Laue class to which it belongs. We thus obtain Table 5.2. Table 5.2: The 11 Laue classes. Each class is surrounded by a thick line. 1

– 1

2

m

2 — m

222

mm2

mmm

4

– 4

4 — m

422

4mm

3

– 3

32

3m

– 3m

6

– 6

6 — m

622

6mm

23

– m3

432

– 43m

– m3m

– 42m

4 — mm m

– 62m

6 — mm m

3. Crystal diﬀraction can be described, as in Section 3.2.1, through the condition that the scattering vector be a reciprocal lattice vector h∗ = ha∗ + kb∗ + lc∗ where a∗ , b∗ , c∗ are the basis vectors of the reciprocal lattice. It is often convenient to describe it as mirror reﬂection oﬀ the lattice planes (hkl), but selective reﬂection because it only occurs when the wavelength satisﬁes Bragg’s law. This is why crystal diﬀraction is often referred to as Bragg reﬂection.

Chapter 5 – Point groups

107

5.8. Plane point groups It is useful, both for later discussions on lattices, and for surface crystallography, to determine the plane crystallographic groups. Their determination can be performed in the same way as for 3-dimensional groups, by looking for the proper groups, then the improper groups. The operation of symmetry with respect to a given point O in the plane is identical to a rotation by 180◦ around an axis perpendicular to the plane that goes through O. It is no more an improper operation. The basic improper operation is now the operation of symmetry with respect to a plane perpendicular to the plane of the object, or mirror operation, noted m. All the plane symmetry elements are perpendicular to the reference plane. The only proper plane crystallographic groups are 1, 2, 3, 4, 6. The improper groups are obtained by multiplying these proper groups with group (E, m). We then obtain groups m, 2m or mm,4 3m, 4m, 6m. We note that these 10 plane crystallographic point groups are identical to 10 of the 3-dimensional point groups.

5.9. Isotropy point groups The investigation of the physical properties of crystals will beneﬁt from a generalization of the discussion in this chapter to inﬁnite-order non-crystallographic point groups. These are groups featuring an axis of revolution, which is none other than an inﬁnite-order axis, or isotropy axis. It will be performed according to the same rules. The result is given below. For each of these groups, we give an example of an object with the symmetry elements of the group (Fig. 5.18).

Proper groups (a) There is a single isotropy axis, and no other symmetry operation. The group has for its symbol ∞. It corresponds to the cyclic groups (Sect. 5.4.2). This is the symmetry of a half cone rotating around its axis. (b) There is a single isotropy axis and an inﬁnity of 2-fold axes perpendicular to it. This group is noted ∞2, and it corresponds to the dihedral groups of Section 5.4.3. This is the symmetry of two half-cones with the same apical angle and with the same axis, but opposed at the apex and rotating in opposite directions.

4. This group contains the symmetry operations associated to a 2-fold axis and a mirror going through this axis. The existence of these two symmetry elements entails the existence of another mirror going through the axis and perpendicular to the ﬁrst one. This is why this group is usually called mm.

108

Symmetry and Physical Properties of Crystals

2

— m

m — m

— m— m

m

(a)

(b)

(c)

(d)

(e)

(f)

(g)

Figure 5.18: Examples of objects having the symmetry of each of the 7 isotropy groups (c) There is an inﬁnity of isotropy axes. This group, noted ∞ ∞, is the limiting case of groups involving several axes of order larger than 2 (corresponding to the cubic proper groups of Sect. 5.4.4). This is the symmetry of a sphere containing a liquid featuring rotatory power, hence not superimposable with its mirror image.

Improper groups containing inversion We multiply by (E, I) the groups obtained in (a), (b) and (c). Since these groups contain at least one isotropy axis (which therefore includes a 2-fold axis), the presence of the center of symmetry is equivalent to the existence of a mirror perpendicular to the axis. We obtain: (d) one isotropy axis and a perpendicular mirror, i.e. the group ∞/m (corresponding to groups 2/m, 4/m, 6/m). This is the symmetry of a cylinder rotating around its axis, and also that of an axial vector (Sect. 10.6.1). (e) one isotropy axis, an inﬁnity of mirrors going through this axis, and a mirror perpendicular to the axis (and a center of symmetry). This group is called ∞/mm (it can be associated to groups 4 ⁄ mmm and 6 ⁄ mmm). This is the symmetry of a stationary cylinder. (f) an inﬁnity of isotropy axes, an inﬁnity of mirrors (and a center). This group is noted ∞/m ∞/m. This is the symmetry of a sphere.

Improper group which does not contain inversion (g) Group ∞2 admits group ∞ as its half order subgroup. The process described for the crystallographic groups now reduces to replacing the inﬁnity of 2-fold axes by an inﬁnity of mirrors going through the isotropy axis. This group is called ∞m. It generalizes the pyramidal groups. This is the symmetry of a stationary half-cone, and also that of a polar vector (Fig. 9.2).

Chapter 5 – Point groups

109

These groups can be classiﬁed into two systems: the cylindrical system, which contains a single axis of revolution (a, b, d, e and g) and the spherical system which contains an inﬁnity of axes of revolution (c and f). These inﬁnite-order groups will be used in the second part of the book to characterize the symmetry of some physical quantities. For example an electric ﬁeld has for its symmetry group ∞m, a magnetic ﬁeld ∞/m and a uniaxial stress (which will be deﬁned in Sect. 11.5.1) ∞/mm.

5.10. Exercises Exercise 5.1 Consider two axes x x and y y, intersecting at point O, and enclosing an angle θ. Let A be the operation consisting of a rotation by π around x x and A the operation rotation by π around y y. 1.

Show that the product A A is equal to a rotation by 2θ around an axis that goes through O and is perpendicular to the plane Π formed by x x and y y. Denote this operation as R⊥ (2θ).

2.

Deduce that A = R⊥ (2θ)A and A = A R⊥ (2θ), so that, if an object features an n-fold axis and a 2-fold axis perpendicular to it, then it also features n 2-fold axes with angles π/n between them.

Exercise 5.2 Consider the point group 32, i.e. a group comprising the symmetry operations associated to a 3-fold axis and to a 2-fold axis perpendicular to it. Draw the stereographic projection, onto a plane perpendicular to the 3-fold axis, of the directions equivalent to a general direction through these symmetry operations. Deduce that this group includes three 2-fold axes perpendicular to the 3-fold axis, with angles of 2π/3 between them. This is an easy way of retrieving the result of the preceding exercise in the special case where n = 3. It can be easily generalized to any value of n. Exercise 5.3 1.

Show that the existence of two intersecting and perpendicular 4-fold axes leads to the existence of four 3-fold axes parallel to the major diagonals of a cube with sides parallel to the 4-fold axes. The derivation can be made either using the rotation matrices representing the symmetry operations, or by considering a cube ABCDEFGH and submitting it to the successive operations.

2.

Show that the reciprocal proposition is not true. The existence of four 3fold axes along the major diagonals of a cube does not entail the existence of three 4-fold axes parallel to the sides of the cube. It only entails the existence of 2-fold axes parallel to the cube sides.

110

Symmetry and Physical Properties of Crystals

Exercise 5.4 Consider Figure 5A.5b showing the stereographic projection of some of the symmetry elements of a cube. If the projection plane is perpendicular to the basis vector c of a cubic lattice, and if b is the projection of [100], the circular arcs b Fb and b F b are the projections of the diagonal plane (01¯1). Show that the centers of the circles to which these arcs belong are points a and a respectively. √ Note: it may be helpful to note that tan π8 = 2 − 1, a value which can be 2 tan θ π retrieved using tan 2θ = 1−tan 2 θ and tan 4 = 1. Exercise 5.5 Consider the various point groups consistent with a hexagonal lattice, and rank them according to their merohedry. Figure 5.17b can be useful. Exercise 5.6 A form {hkl} of a crystal comprises the set of faces in this crystal which are equivalent to face (hkl). 1.

Give the Miller indices of the various planes in the form {31¯40} for crystals with point group (a) 6mm, then (b) ¯62m.

2.

Same question for form {111} in crystals belonging to the various cubic groups.

Chapter 5 – Point groups

111

Appendix 5A. Complements on the stereographic projection 5A.1. Stereographic projection of the transform of a given direction through the symmetry operations associated to various symmetry elements The notations are as follows. We call Ov the starting direction. It intersects the sphere at P, the stereographic projection of which is called n. Direction Ov , the transform of Ov through the considered symmetry operation, cuts the sphere at P , and its stereographic projection is called n . The meridian half-planes containing OP and OP intersect the projection plane along OQ and OQ respectively (Fig. 5A.1). Projections n and n are then located on OQ and OQ respectively. v’ N

N

Q’

P’

v P O

n

n’ Q

O

n’

Q’

O n Q

S

S

(a)

(b)

(c)

Figure 5A.1: Illustrating the notations used in this appendix: (a) meridian plane of the initial direction Ov ; (b) meridian plane of direction Ov , the transform of Ov through the symmetry operation; (c) stereographic projections n and n of directions Ov and Ov 5A.1.1. n-fold axis perpendicular to the projection plane The projection of the axis consists of two points coinciding with the origin O. The meridian planes containing Ov and Ov enclose an angle 2π/n. Ov and Ov are at the same angle θ to NS and On = On . Projection n is the transform of n through a rotation by 2π/n around an axis perpendicular to the projection plane and going through O (Fig. 5.2 and 5.4). 5A.1.2. Mirror coinciding with the equatorial plane The stereographic projection of the mirror is the equatorial circle. The meridian plane containing Ov transforms into itself in the mirror operation, and in this plane Ov and Ov are symmetric with respect to the trace of the equatorial plane (Fig. 5A.2a). The projections coincide but they are represented by diﬀerent signs since Ov and Ov are in two diﬀerent hemispheres (Fig. 5A.2b).

112

Symmetry and Physical Properties of Crystals N v P n n’

O

n’ n

7

O

QQ’ P’

Q

v’

S

(a)

(b)

Figure 5A.2: (a) Meridian plane containing a general direction Ov and its transform Ov through symmetry with respect to a mirror coinciding with the equatorial plane; (b) stereographic projections of the mirror (thick line) and of directions Ov and Ov 5A.1.3. Mirror going through axis NS The projection of the mirror is the line AB, intersection of the mirror and the equatorial plane (Fig. 5.3b). The meridian plane containing OP is symmetric of the one containing OP with respect to the mirror plane. In each of these planes, OP and OP enclose the same angle θ with axis NS, so that On = On . Their stereographic projections n and n are therefore symmetric with respect to the stereographic projection of the mirror. 5A.1.4. 2-fold axis in the equatorial plane The projection of the axis consists of two opposite points on the equatorial circle, A and B (Fig. 5A.3c). Direction Ov intersects the sphere at point P, which projects on the equatorial plane at H. The meridian plane containing Ov is at an angle ϕ with AB. The transform of this meridian plane through a rotation by π around AB is a meridian plane enclosing the same angle ϕ with AB. The transforms of P and H are P and H respectively, and it is easy to show, using Figure 5A.3a, that (OH, OP) = (OH , OP ) = β, P being in the northern hemisphere and P in the southern hemisphere. The stereographic projections n and n are therefore at the same distance from O on OQ and OQ (Fig. 5A.3b), both of which enclose with AB the angle ϕ. They are represented with diﬀerent symbols (Fig. 5A.3c).

5A.2. Stereographic projections of the symmetry elements of a cube 5A.2.1. Preamble We look for the stereographic projection of a plane going through the center O of the sphere and which does not go through axis NS. Its intersection with the sphere is a major circle Γ which intersects the equatorial circle at a and a (Fig. 5A.4a).

Chapter 5 – Point groups

113

v P C

A

O

H

Q A2 axis B

H’

P’

Q’ v’

(a) N

Q’ H’

n’

N

OO

P

n

H

Q

v

n O

A

n’

v’ P' S

Q B Q’

S

(b)

(c)

Figure 5A.3: Construction of the stereographic projection of the transform of a general direction Ov through rotation by π around an axis A2 located in the equatorial plane: (a) perspective view; (b) meridian planes containing Ov and Ov ; (c) stereographic projection

N 2 a’

O

a

C

a’

a

1

S (a)

(b)

Figure 5A.4: A plane which does not go through axis NS. (a) Perspective view. (b) The stereographic projection of the plane consists of two arcs in full and dotted thick line, going through a and a .

114

Symmetry and Physical Properties of Crystals

The stereographic projection of a circle being a circle, the projection of Γ starting from the south pole is a circle Γ1 going through a and a (Fig. 5A.4b). This circle has two parts: arc aa’ (thicker line), located in the equatorial disk C, which corresponds to the projection of the half major circle located in the northern hemisphere. The second half of major circle Γ, located in the southern hemisphere, must be transformed through an inversion with the north pole as pole. The transform of Γ through the north pole inversion is circle Γ2 , symmetric of Γ1 with respect to aa , with only the circular arc contained in the equatorial disk retained. It is represented in dotted line to indicate that it is the image of an arc in the southern hemisphere. 5A.2.2. Cubic groups The stereographic projection is performed onto a plane parallel to one cube face, for example face HJKL of the cube shown on Figure 5A.5a. 1.

Stereographic projection of one of the A3 axes of the cube Select for example the A3 axis coinciding with the major diagonal HK . This diagonal is at the intersection of two diagonal planes of the cube, HJK L and HLK J . The stereographic projection of plane HJK L consists of two arcs intersecting along diameter aa parallel to HJ. That of plane HLK J consists of two arcs intersecting along bb parallel to side HL (Fig. 5A.5b). The stereographic projections of the axis are the intersections of the stereographic projections of the two diagonal planes, i.e. point F is in the northern hemisphere and point F in the southern hemisphere. They are represented by their characteristic symbol (an equilateral triangle). Axis A3 is contained in a third diagonal plane of the cube, HKK H . This plane goes through axis NS. Its projection coincides with its intersection with the projection disk, i.e. the segment cc at 45◦ to aa and bb . It goes through F and F .

2.

Stereographic projection of all the symmetry elements of the cube, i.e. of the point group m¯3m (Fig. 5A.5c) The three A4 axes represented by their characteristic symbols. The mirrors perpendicular to these A4 axes, i.e. the mirror parallel to the projection plane (and to face HJKL), the projection of which is the equatorial circle itself, and the mirrors parallel to axis NS, the projections of which are the segments aa and bb (mirrors parallel to HJJ H and JKK J respectively). The diagonal mirrors. There are six of them. We investigated three of them, which intersect along an A3 axis. To each of these three mirrors we can associate another diagonal mirror which is perpendicular to it and intersects it along an A4 axis. For example, mirror LJJ L is associated to mirror HKK H . These two mirrors go through axis NS and their stereographic projections are cc and dd . Mirror H J KL is

Chapter 5 – Point groups

115

associated to HJK L . They are symmetric of each other with respect to the projection plane. Their stereographic projections are identical (arcs aFa and aF a ), but with the characteristic symbols reversed. The arc in full line of one is superimposed on the arc in dotted lines of the other, and vice-versa. Finally the full lines cover the dotted lines. The same applies to the projections of the diagonal mirror HLK J and H L KJ, which consist of the arcs bFb and bF b . Six A2 axes perpendicular to the diagonal mirrors, and therefore located in the associated diagonal mirror. They connect, within these mirrors, the middles of two opposite sides. For example MP, located in the diagonal mirror HJK L , is the A2 axis perpendicular to mirror H J KL. Its stereographic projection consists of two points G and G’ (Fig. 5A.5b). The axis A2 located in the mirror H J KL projects on the same points but with diﬀerent symbols. On the general ﬁgure, we show these two axes (as well as the four others) using the representative symbols of 2-fold axes. A center of symmetry. Its stereographic projection is at the center of the projection disk. Furthermore, the presence of a center of symmetry changes the A3 axes into ¯3-fold axes. L’

P K’

H’ O

J’

L K

H M

J

(a) b’

b’ d’

c’ G

a F’

c’

F G’

c

a’

a

a’ d

c b (b)

b (c)

Figure 5A.5: (a) Perspective view of a cube; (b) stereographic projection of some of its symmetry elements and (c) of all its symmetry elements

Chapter 6

Bravais lattices This chapter shows how the Bravais lattices, already introduced in a qualitative way in Section 3.7, are enumerated. It can be skipped on ﬁrst reading.

6.1. Introduction Bravais lattices were introduced in Section 3.7. We showed that, in some cases, a multiple (or centered) cell evidences symmetry elements of the lattice which fail to appear in any primitive cell. We listed the 14 Bravais lattices (Sect. 3.7.2 and Tab. 3.3), without deriving how they are enumerated. The aim of the present chapter is to show how they are obtained logically. It can therefore be skipped on ﬁrst reading. The derivation rests on the result obtained in Section 4.3, namely that the symmetry operations of the point group of the crystal form a subgroup of the symmetry operations of the crystal lattice. The aim is therefore to ﬁnd out what type of crystal lattice is consistent with each of the 32 point groups. However, since all crystal lattices feature centers of symmetry (on the nodes, at the centers of the unit cells and in the middle of the vectors connecting neighboring nodes), the point symmetry group of a crystal lattice necessarily contains inversion. It is therefore suﬃcient to know the lattice types consistent with each of the 11 centrosymmetric point groups, each of which is characteristic of its Laue class, deﬁned in Section 5.7. The lattices of the 21 other groups are obtained by considering, for a given group, the group representative of its Laue class, i.e. the supergroup obtained by multiplying it with the group (E, I). This supergroup is one of the 11 centrosymmetric groups for which we determined the compatible lattice. In practice, we will use this remark only in the course of the derivation, because it is simpler to start out by determining which lattice is consistent with a low-symmetry point group. We will see that we reach a lattice for which the point group is much more symmetric than the starting group, and therefore necessarily includes a set of subgroups. Before that, it is necessary and illuminating to enumerate the plane lattices. The results obtained are no surprise; they were already given without derivation in Section 3.4.1.

© Springer Science+Business Media Dordrecht 2014 C. Malgrange et al., Symmetry and Physical Properties of Crystals, DOI 10.1007/978-94-017-8993-6_6

117

118

Symmetry and Physical Properties of Crystals

6.2. Plane lattices We recall that the 10 plane point groups are the groups 1, 2, 3, 4, 6, m, mm,1 3m, 4m, 6m (Sect. 5.8). We will investigate successively the plane lattices compatible with the low-symmetry point groups, viz. groups 1, 3, 4 and m. The results obtained make it possible to determine the plane lattices consistent with each of the 10 groups.

6.2.1. Group 1 The point group of any (general) plane lattice features a center of symmetry, i.e., in terms of plane groups for which the symmetry elements are normal to the plane, a 2-fold axis. The unit cell is a general parallelogram, a result valid for groups 1 and 2.

6.2.2. Group 3 Let a be the smallest of all lattice translations. Through a rotation by 2π/3 around the 3-fold axis, vector a becomes vector b (Fig. 6.1a). Vectors a and b deﬁne a primitive cell, since there cannot be a node within this parallelogram, or else a would not be the smallest lattice vector. Only one type of plane lattice is consistent with a 3-fold axis. Its primitive cell is a parallelogram with apical angles 2π/3 and π/3, and the lattice is called hexagonal. The symmetry of this lattice is 6m and the point groups consistent with this lattice are thus 3, 3m, 6, 6m (Fig. 6.1b).

b

120°

O

a b

120°

a

(a)

(b)

Figure 6.1: Plane lattice with point group 3: (a) primitive cell; (b) lattice, evidencing six concurrent mirrors, the trace of which is indicated by dotted lines

1. We saw that this notation is equivalent to the notation 2m.

Chapter 6 – Bravais lattices

119

6.2.3. Group 4 The same argument (rotation by 2π/4 = π/2 of the smallest lattice vector a, leading to vector b deﬁning, together with a, a square unit cell within which there can be no extra node) leads to a square primitive cell. The plane lattice, with square primitive cell, has point symmetry 4m and is consistent with the point groups 4 and 4m.

6.2.4. Group m Let a be a translation of the plane lattice that is neither parallel nor perpendicular to the trace uu of the mirror on the plane of the lattice, and b the transform of a in the mirror operation m (Fig. 6.2a). Translations a + b and a − b deﬁne orthogonal rows, respectively parallel and perpendicular to the mirror. Let a and b be the smallest lattice vectors along these directions (Fig. 6.2b). They deﬁne a rectangular unit cell for which one of the apices is noted O. Consider a lattice vector n starting from O and for which the end M is inside the rectangle deﬁned by the vectors a and b with origin O. Let n = OM be its image through operation m. Draw the vector n + n , parallel to b. By construction, it is smaller than 2b and can only be a multiple of b, i.e. 0 or b. In the same way, n − n can only be 0 or a. u’

a’ + b’ b’

a’

b M

M’ n’

a’ – b’

O

n a

u

(a)

(b)

Figure 6.2: Plane lattice with point group m. uu’ is the trace of one of the mirrors. Consider the various possible cases: 1.

n + n = 0 and n − n = 0, i.e. n = n = 0. The rectangular unit cell with basis vectors a and b is primitive.

2.

n + n = b and n − n = a, i.e. n = (a + b)/2. The rectangular unit cell is double. It is a centered unit cell.

3.

n + n = b and n − n = 0, i.e. n = b/2 or n + n = 0 and n − n = a, i.e. n = a/2.

120

Symmetry and Physical Properties of Crystals

These two solutions must be rejected because they contradict the starting assumption (a and b the smallest lattice vectors along these directions). These two plane lattices, with the rectangular unit cell respectively primitive and centered, have point symmetry mm, and the compatible crystal groups are m and mm.

6.2.5. Conclusion The survey of plane lattices is ﬁnished because, by searching for the lattices associated with the lowest symmetries, we have determined lattices with higher symmetry which ﬁnally include all the plane point groups. The results are gathered in Table 6.1. Table 6.1: Point groups consistent with the various plane lattices Plane lattice

Compatible point groups

Oblique

1, 2

Hexagonal

3, 3m, 6, 6m

Square

4, 4m

Rectangular Primitive (p) Centered (c)

m, mm

6.3. 3-dimensional lattices 6.3.1. Group 1 This group features no symmetry element. It is therefore consistent with a general parallelepiped-shaped primitive cell. The lattice is called triclinic. As for all lattices, it involves centers of symmetry and its point group is thus ¯1. It is therefore consistent with crystals with point groups 1 and ¯1.

6.3.2. Group 2 We showed (Sect. 3.3.4) that any rotation axis is parallel to a row of the direct lattice and perpendicular to a lattice plane. Consider row zz parallel to the 2-fold axis, and going through a given lattice node O. Let P0 be the lattice plane which is perpendicular to this row and goes through O (Fig. 6.3). In plane P0 , the primitive cell is a general parallelogram. Let a and b be two vectors deﬁning this unit cell. Let P1 be one of the two lattice planes parallel to P0 and closest to P0 . The lattice nodes in this lattice plane project onto P0 at the rate of one node per plane unit cell in P0 . Let F be the projection of one of these nodes, located in

Chapter 6 – Bravais lattices

121 z’

F

P1

b a

n B P0

O

F’

A

D

z

Figure 6.3: Three-dimensional lattice for a crystal with point group 2. zz is a 2-fold axis. P0 and P1 are two consecutive lattice planes. Vector n = OF connects node O in P0 to a node of plane P1 such that its projection is inside the plane unit cell OADB. one of the unit cells containing lattice node O, and let F be the node associated to it in P1 . F can also be located on the edges OA and OB of this unit cell, but A and B are excluded: if F were at A (or B) we would consider OF − a (or OF − b) and F would then be at O. Let us note vector OF as n. The three vectors a, b and n deﬁne a primitive cell. Let n be the lattice vector resulting from the transformation of n through a rotation by π around the 2-fold axis (Fig. 6.4a). The component n// of n, parallel to the axis, is conserved in the rotation, and the component n⊥ is transformed into −n⊥ . Also, n − n is a lattice vector. We obtain: n = n// + n⊥ ,

n = n// − n⊥ ,

n − n = 2n⊥ = pa + qb

(p and q integers)

Hence n⊥ =

q p a + b. 2 2

(6.1)

Taking into account the assumption we made about F and F , p/2 and q/2 are less than 1. Two cases must be considered: 1.

n⊥ = 0 (p = q = 0), so that n is perpendicular to P0 . The unit cell is a right prism with general parallelogram base. It is a primitive cell and the lattice is called monoclinic primitive.

2.

n⊥ = a/2 or n⊥ = b/2 or n⊥ = (a + b)/2. These three cases are equivalent, since nothing basically distinguishes lattice vectors a, b and a + b, any one of which can be chosen as a basis vector for a plane primitive cell in P0 .

Assume that n⊥ = a/2 (Fig. 6.4b). Plane P2 , parallel to P0 and P1 and located immediately above P1 , deduces from P0 through translation 2n, i.e.

122

Symmetry and Physical Properties of Crystals z’

z’ c = 2n F

n

n n’

2n F n b

b n a

O

F’

P0

O a/2 F’ a P0

z

z

(a)

(b)

Figure 6.4: Search for the lattice of a crystal with point group 2. (a) Vector n transforms into n by rotation around the 2-fold axis zz . (b) The situation when the component n⊥ of n perpendicular to zz is equal to a/2. 2n = 2n// + a, which is equal to 2n// modulo the lattice translations. The vectors a, b and c = 2n// deﬁne a monoclinic unit cell. This unit cell contains node F at the center of the rectangular face (a, c = 2n// ). It is a double unit cell, called base-centered monoclinic. The centered faces are parallel to the 2-fold axis. If, as we just did, we call c the basis vector parallel to the 2-fold axis, the lattice is called monoclinic B if the centered faces are (a, c), or monoclinic A if the centered faces are (b, c). If, as is still frequently the case, the basis vector parallel to the 2-fold axis is called b, the lattice is C or A depending on whether faces (a, b) or (b, c) are centered. The point group of a monoclinic lattice is 2/m. It is consistent with subgroups 2 and m and with group 2/m.

6.3.3. Group 3 In the lattice planes perpendicular to the 3-fold axis, the lattice is hexagonal. It is deﬁned by vectors a and b, with the same length and enclosing an angle 2π/3. The same argument as above leads to considering a lattice plane P0 perpendicular to the 3-fold axis, and its nearest neighbor P1 , which is parallel to it. Let n be the lattice vector connecting lattice node O in plane P0 to lattice node F located in P1 and which projects onto P0 inside a primitive plane unit cell containing O, or one of its sides OA and OB, excluding A and B. Let n be the transform of n through the operation rotation by 2π/3 around the 3-fold axis going through O. The component n// of n parallel to the axis is conserved in the rotation. n = n// + n⊥ ,

n = n// + n⊥ ,

where n⊥ and n⊥ are respectively the components of n and n perpendicular to the 3-fold axis (Fig. 6.5).

Chapter 6 – Bravais lattices

123 B

D b F’

n

n’ O

a

A

Figure 6.5: Primitive cell in plane P0 perpendicular to the 3-fold axis Taking into account the assumption made about F , the end of n⊥ is located inside the parallelogram OADB (or on OA or AB, excluding A and B) and thus its norm is smaller than a. We have ||n⊥ || < a. Since n⊥ − n⊥ =

√

√ 3 n⊥ , we obtain n⊥ − n⊥ < a 3.

As n − n is a lattice vector, n⊥ − n⊥√ , which is equal to it, is also a lattice vector, the norm of which is less than a 3. This norm can therefore have only two values, 0 or a. 1.

n⊥ − n⊥ = 0, so that n⊥ = n⊥ = 0. Vector n is perpendicular to P0 and the unit cell is a right prism whose base is an isosceles parallelogram with apical angle 2π/3. The unit cell is primitive, and the lattice is called hexagonal primitive. The point group of such a unit cell is 6/mmm, of which 3 is a subgroup (of index 8). The hexagonal lattice is therefore consistent also with groups 3, ¯3, 32, 3m, ¯3m, 6, ¯6, 6/m, 622, 6mm, ¯62m, subgroups of 6/mmm. This result was shown on Figures 5.17a and 5.17b.

2.

n⊥ − n⊥ = a, and then n⊥ − n⊥ is a lattice vector in P0 , with length a. It is therefore equal to a or b or a + b. Assume it is equal to a (Fig. 6.6a). The end F of n⊥ is then at the center M of the equilateral triangle OAD, and the nodes of the plane lattice P1 project at M and at all the points deduced from M through lattice translations a and b, thus, for example, at N and P. The lattice of plane P2 , immediately above P1 , deduces from the lattice of plane P0 through translation 2n = 2n// + 2n⊥ , and its nodes project onto P0 at N, such that ON = 2OM, and at all the points deduced from N through the lattice translations, for example at Q, R and S.

The lattice in plane P3 immediately above P2 is deduced from that of P0 through translation 3n = 3n// + 3n⊥ . But 3n⊥ = OK, a lattice vector equal to 2a + b. The nodes of plane P3 project on the nodes of P0 . Comparing Figures 6.6a and 3.14c, we see that the unit cell is a rhombohedron (Fig. 6.6b), i.e. a parallelepiped for which the basis vectors a , b and c have the same length, and for which the major diagonal LT is a 3-fold axis. All its faces are lozenges, equal to one another. The point group of a rhombohedral unit cell is ¯3m. Such a lattice is therefore consistent with the point group ¯3m and its subgroups 3, ¯3, 32, 3m.

124

Symmetry and Physical Properties of Crystals T B

D b

N

K N

R

n’ O

n a

S

R’

S’

M A

N’

Q

M’

P’ c’

P

Q’

a’

b’

L

(a)

(b)

Figure 6.6: Rhombohedral lattice: (a) projection onto plane P0 of the lattice nodes; (b) rhombohedral unit cell. P , M , N are in plane P1 and project onto P0 at P, M and N (crosses); Q , R , S are in plane P2 and project onto P0 at Q, R and S (empty circles); T is in plane P3 and projects at O (full circle). We thus obtained the two following results: 1.

¯ 32, 3m and ¯3m are consistent with a The crystals with point group 3, 3, primitive rhombohedral crystal lattice, noted R, and also with a primitive hexagonal lattice, noted P. Some crystals with one of these point groups have a rhombohedral lattice while others have a hexagonal lattice. For example, crystals of calcite CaCO3 , with point group ¯3m, have a rhombohedral lattice while crystals of Ca(OH)2 , with the same point group, have a hexagonal lattice.

2.

The hexagonal lattice is consistent with groups 6, ¯6, 6/m, 622, 6mm, ¯62m and 6/mmm. It will therefore not be necessary to examine group 6.

6.3.4. Group 4 Plane P0 , perpendicular to the 4-fold axis, is a lattice with a square primitive cell, with basis vectors a and b with the same norm a. The same argument as for groups 2 and 3 leads to considering the vector n connecting lattice node O in P0 to node F in lattice plane P1 (parallel to P0 and nearest neighbor to it) which projects onto P0 at point F (Fig. 6.7a), located within the plane unit cell OADB (or on OA and OB, excluding A and B). Let n be the transform of n through rotation by π/2 around the 4-fold axis. The component n// of n parallel to the axis is conserved in the rotation. We have n = n// + n⊥ , and

n = n// + n⊥ n⊥ = n⊥ .

√ Also, the assumption made on F leads to n⊥ < a 2.

Chapter 6 – Bravais lattices

125

c = 2n B

D

B

b n’

b

n O

F’ a

(a)

Figure 6.7: (a) Plane P0 , n⊥ through a n⊥ − n⊥ = a. Thus and

n

F’ B

n

n’ A

F

D

O

a

D F’

A

O

A

(b)

Search for the lattice of a crystal with point group 4. perpendicular to the 4-fold axis: n⊥ is the transform of rotation by π/2 around the 4-fold axis. (b) Case where The end of vector n = OF is at the center of the unit cell. n − n = n⊥ − n⊥ √ n⊥ − n⊥ = n⊥ 2.

Therefore n − n , and n⊥ − n⊥ which is equal to it, are lattice vectors parallel to P0 with norm smaller than 2a. Two cases should be distinguished: 1.

n⊥ − n⊥ = 0, so that n⊥ = n⊥ = 0 and n = n = n// . The unit cell is primitive. It is a rectangle parallelepiped with square base. The unit cell is called tetragonal primitive.

2.

n⊥ − n⊥ = a so that n⊥ = (a + b)/2. There is a lattice node which projects at the center of the square plane unit cell OADB (Fig. 6.7b). The plane P2 , nearest neighbor to P1 , deduces from P0 through translation 2n = 2n// + a + b. The nodes of P2 therefore project on the nodes of P0 . The lattice has a tetragonal double unit cell, with a node at the center of the unit cell.

This is a tetragonal body-centered lattice, noted I. The point group of a tetragonal unit cell is 4/m mm. This unit cell is consistent with point groups 4, ¯4, 4/m, 422, 4mm, ¯42m and 4/m mm. A tetragonal unit cell can therefore be primitive (P) or body-centered (I). It is then unnecessary to deal with group 6, since it occurred in a natural way when considering group 3 (Sect. 6.3.3). The above discussions led to the determination of the lattices consistent with 24 of the 32 point groups. We now search for the lattice consistent with the least symmetric of the remaining point groups, viz. 222.

126

Symmetry and Physical Properties of Crystals

6.3.5. Group 222 This group features three 2-fold axes, perpendicular to one another. Each of these axes being parallel to a lattice row (Sect. 3.3.4), the unit cell, be it primitive or centered, is therefore a rectangle parallelepiped with basis vectors a, b, and c, orthogonal to one another. The lattice is called orthorhombic. Consider the 2-fold axis parallel to vector c. The lattice plane perpendicular to c has a rectangular unit cell which, as we saw in Table 6.1, can be either primitive or centered. We will therefore successively apply the result of Section 6.3.2 to each of these unit cells. The plane unit cell (a, b) is primitive (plane lattice p) The approach of Section 6.3.2 leads to the result given in Equation (6.1): n⊥ =

q p a + b. 2 2

Three cases must be considered: 1.

p = q = 0, so that n⊥ = 0. The unit cell is primitive.

2.

p = 1, q = 0 or p = 0, q = 1, so that n⊥ = a/2 or b/2. The lattice is base-centered B or A. The unit cell is double.

3.

p = 1, q = 1, so that n⊥ = (a + b)/2. The lattice is body-centered, i.e. I. The unit cell is double.

The plane unit cell (a, b) is centered (plane lattice c) We can choose as basis vectors of a primitive cell of the 2-dimensional lattice a and (a + b)/2. We then obtain n⊥ =

q p a + (a + b) 2 4

with p and q integers. The cases to be considered are: 1.

p = 0, q = 0 so that n⊥ = 0. The lattice is base-centered, with the centered base being (a,b), and the lattice is C-type.

2.

p = 1, q = 0, so that n⊥ = a/2. The face (a, c) is centered. Vector (a + c)/2 is a lattice translation. Since face (a, b) is centered, (a + b)/2 is also a lattice vector and, through addition modulo a lattice vector, so is (b+c)/2. All the faces are centered, and the lattice is face-centered (F) orthorhombic.

3.

p = 0, q = 1, so that n⊥ = (a + b)/4.

4.

p = 1, q = 1, so that n⊥ = (3a + b)/4.

Chapter 6 – Bravais lattices

127

Cases (3) and (4) are to be rejected, since they lead to lattices that do not accept a 2-fold axis parallel to a or b. In conclusion, the orthorhombic lattice can be primitive (P), base-centered (A, B or C), body-centered (I) or face-centered (F). The orthorhombic lattice has symmetry mmm, and it is therefore consistent with groups 222, mm2 and mmm.

6.3.6. Group 23 Among the remaining groups, the least symmetric one is group 23. It is a supergroup of 222, which means that it features all the symmetry operations of 222, with additional 3-fold axes. This implies that the lengths of basis vectors a, b and c are equal. We can therefore start out from the results obtained for 222, adding the equality of the lengths of a, b and c. The unit cell is a cube which can be primitive (P), body-centered (I) or face-centered (F). The A, B and C lattices are not consistent with the existence of 3-fold axes, and are therefore ruled out. The lattice is cubic. The point group of the lattice is m¯3m and the cubic lattice is consistent with groups 23, m¯3, 432, ¯43m and m¯3m. We have now gone through the full list of crystallographic point groups, and the overall result is shown in the last column of Figures 5.17a and 5.17b.

Chapter 7

Space groups After showing how the space groups are constructed, this chapter aims at enabling the reader to understand what the denomination of a given space group contains, and to eﬃciently use volume A of the International Tables for Crystallography. This volume lists all the space groups and gives many of their properties. The last section shows some examples of space groups.

7.1. Introduction We saw that the symmetry operations of a crystal can be expressed in the form (S, t) where S is a rotation or a rotoinversion about an axis going through a given point O, and t a translation. Point O is not explicitly mentioned in the notation because it is chosen as common to all the operations (S, t). We also saw that the symmetry of the physical properties of a crystal depends only on the operations S, which form a group, and, in Chapter 5, we enumerated the 32 symmetry groups of the operations S, called orientation groups or, more often, point groups. We must now enumerate the symmetry groups of the operations (S, t). The connection between the point group and the space group was established rigorously in Chapter 4. We recall it brieﬂy here. The group T of the lattice translations (E, n) where E is the identity operation and n a vector of the crystal lattice, n = ua + vb + wc (a, b and c are the basis vectors of the crystal unit cell and u, v, w any integers), is a subgroup of the group G of the symmetry operations of the crystal. We can decompose this group G into packets (or cosets), each of which is the product of an operation (Si , ti ) with all the translation operations, so that: G = T + T(S1 , t1 ) + T(S2 , t2 ) + T(S3 , t3 ) + . . . + T(Sm , tm ) = T(E, 0) + T(S1 , t1 ) + T(S2 , t2 ) + T(S3 , t3 ) + . . . + T(Sm , tm ). To perform this partition of G by the group T of lattice translations, we start by setting aside the group T. We choose among the remaining elements of G one operation (S1 , t1 ), and we perform all the products of this operation with © Springer Science+Business Media Dordrecht 2014 C. Malgrange et al., Symmetry and Physical Properties of Crystals, DOI 10.1007/978-94-017-8993-6_7

129

130

Symmetry and Physical Properties of Crystals

the lattice translations. This set T(S1 , t1 ) is then put aside, and the process is repeated until all the elements of G have been used. The vectors ti are deﬁned modulo the lattice translation vectors. We can therefore choose them either equal to zero, or equal to pa + qb + rc with p, q, and r smaller than 1. The set of the cosets T(Si , ti ) thus deﬁned forms Gs , the space group or position group of the crystal, which can also be written as: Gs = (E, 0) + (S1 , t1 ) + (S2 , t2 ) + (S3 , t3 ) + . . . + (Sm , tm ) (modulo T),1 by replacing each coset T(Si , ti ) by (Si , ti ) modulo T. The operations (Si , 0) obtained by replacing, in (Si , ti ), the translation ti by a zero translation, form the point group or orientation group G0 of the crystal: G0 = (E, 0) + (S1 , 0) + (S2 , 0) + (S3 , 0) + . . . + (Sm , 0). The 32 point symmetry groups compatible with the existence of a crystal lattice were enumerated in Chapter 5. The ﬁrst task in this chapter will be to determine the operations (Si , ti = 0) which can exist when the existence of the crystal lattice is taken into account. We will thus obtain the symmetry operations associated to screw axes and to glide mirrors. We will then show how the space groups can be determined starting from the point groups, but we will not enumerate them systematically. There are 230 of them. They are described in volume A of the International Tables for Crystallography (I.T. A) [1], presented in Section 7.3.3.

7.2. Enumeration of the operations (S, t) We considered till now symmetry operations of the form (S, t) where operations S are rotations (or rotoinversions) around an axis that goes through point O, chosen arbitrarily and common to all the symmetry operations. We showed (Sect. 4.2.1) that this choice of a common point for all the rotation and rotoinversion axes is possible because we may always replace an operation (S(O), t) by an operation (S (O ), t ) where O is any point, if S = S and t = t + (S – E) OO . We now reverse the reasoning, in order to determine whether it is possible, for any one of the operations (S(O), t), with common origin O, to displace the 1. Adding “modulo T” is mandatory in order for the above operations to form a group because it can happen that the product of two of the operations (Si , ti ) is equal to (Sj , tj + n) while, as mentioned above, the ti are smaller than lattice translations.

Chapter 7 – Space groups

131

origin to a point O so that we obtain an operation for which the translation part is zero, (S(O ), 0). To obtain t = 0 we require: t = (E – S) OO .

(7.1)

We will see that this equation can have solutions in some cases. When it does not, we will determine the values of t compatible with the existence of a crystal lattice. We will study separately the cases where S is a rotation (Sect. 7.2.1) ¯ (Sect. 7.2.2). and those where S is a rotoinversion, denoted as above with S

7.2.1. S is a rotation. Deﬁnition of screw axes It is easily shown that, if S is a rotation, the vector t deduced from relation (7.1) is perpendicular to the rotation axis. Rotation S(O) transforms vector OO into vector OO (Fig. 7.1). We obtain: t = (E – S) OO = OO − OO = O O

(7.2)

which is perpendicular to the rotation axis. Thus the translation part of the operation can be zero only if the initial translation t is perpendicular to the rotation axis. z’ O”

O’

O z

Figure 7.1: Rotation of a vector OO around an axis zz that goes through O The determination of the new position O of the axis which cancels the translation will be presented in Section 7.2.3. We now consider the case (S, t// ), where t is parallel to the rotation axis, so that the translation part can no more be canceled by a change in the position of the rotation axis. Suppose S is a rotation by 2π/q around a q-fold axis, and determine the operation product of this operation by itself. Using relation (4.8), valid for operations S1 and S2 having the same origin, which we reproduce below: (7.3) (S2 , t2 )(S1 , t1 ) = (S2 S1 , S2 t1 + t2 ). We obtain: (S, t// ) (S, t// ) = (S2 , St// + t// ).

132

Symmetry and Physical Properties of Crystals

But St// = t// since rotation of a vector parallel to the rotation axis transforms this vector into itself. We obtain (S, t// )2 = (S2 , 2t// ). Repeating this operation q times, we obtain: (S, t// )q = (Sq , q t// ) = (E, q t// ) which is necessarily a symmetry operation of the crystal. Since the rotation part is the identity operation, this symmetry operation is a lattice translation (E, n) and qt// = n. Vector t// is therefore parallel to a crystal row, which is no surprise since it is parallel to a symmetry axis (Sect. 3.3.4). Let c be the smallest lattice vector parallel to the q-fold axis we are discussing. qt// = mc

and

t// = mc/q

where m is any integer. There are q − 1 solutions: t// = c/q, t// = 2c/q, . . . , t// = (q − 1)c/q. The next values would be t// = c, a crystal lattice vector, and then vectors equal to the above ones modulo c. The symmetry elements associated to these operations, products of a rotation and a translation parallel to the rotation axis, are called screw axes (Sect. 2.2.4). Table 7.1 summarizes the various screw axes, their short notation, the translation to which they are associated, and the symbol that represents them. Table 7.1: Screw axes Order of the axis

2

3

4

6 6 61

64

Notation

2 21 3 31

Translation

0 c/2 0 c/3 2c/3 0 c/4 2c/4 3c/4 0 c/6 2c/6 3c/6 4c/6 5c/6

32

4 41

42

43

62

63

65

Symbol

Consider a crystal featuring a screw axis, and a given atom of this crystal which is not located on this axis. There are then atoms of the same nature at all the positions which deduce from the position of this atom through the various symmetry operations associated to this axis. The atoms are located on a helix or screw (hence the name screw axis), the axis of which is this screw axis. A helix or screw is a chiral object, i.e an object which is not superimposable to its mirror image.

Chapter 7 – Space groups

133

c

21

c

31

32 4’ 3

5 2

c

4 1

3’

41

42

43

c

61

62

63

64

65

Figure 7.2: Equivalent positions of a general atom through the symmetry operations associated to the various screw axes. We note that only axes 31 , 32 , 41 , 43 , 61 , 62 , 64 , 65 are chiral. We could therefore assume that the atoms equivalent through the symmetry operations associated to a screw axis form a chiral ﬁgure. But we must consider all the atoms equivalent within the unit cell, i.e. perform the operation modulo c. As a result, the ﬁgure obtained is not always chiral, as Figure 7.2 shows. Consider for example the case of a 42 axis. The 42 operations performed successively on atom 1 lead to atom 2, then to atom 3, then to atom 4 rotated by 3π/2 and translated by 3c/2 with respect to atom 1. The atom equivalent to 4 through a lattice translation operation −c is atom 4. The transform of atom 4 is atom 5. The atom at 3 is the equivalent of atom 3 through translation −c. We see that the equivalent positions produced, within a unit cell, by these operations 42 do not form a helix or screw, and that the ﬁgure features

134

Symmetry and Physical Properties of Crystals

mirror symmetry. In the same way, the ﬁgures associated to axes 21 and 63 (i.e. axes qm where q = 2m) are not chiral. We note that, among the chiral ﬁgures, those associated to axes 31 , 41 , 61 and 62 are respectively symmetric through a mirror operation of the ﬁgures associated to axes 32 , 43 , 65 and 64 . These ﬁgures are said to be enantiomorphic of each other.

¯ Deﬁnition of glide mirrors 7.2.2. S is a rotoinversion, noted S. We proceed in the same way as for rotations, i.e. we ﬁrst look whether a change in position of the rotoinversion axis makes it possible to reduce the translation to zero. Equation (7.1) is ¯ OO = t (E − S)

(7.4)

which we now solve, not geometrically as was done for rotations, but through ¯ is a rotation S followed by matrix algebra. We recall that rotoinversion S ¯ inversion, S = IS. We choose a system of axes Oxyz such that axis Oz coincides with the rotation axis, and O is the inversion center. In this axis system: ⎛ ⎞ − cos ϕ sin ϕ 0 0⎠ , S¯ = IS = ⎝ − sin ϕ − cos ϕ 0 0 −1 ⎛ ⎞ 1 + cos ϕ − sin ϕ 0 E − S¯ = ⎝ sin ϕ 1 + cos ϕ 0 ⎠ . 0 0 2 In order for Equation (7.4) to have a solution for all t, the determinant of ¯ det(E − S), ¯ must be non-zero. E − S, ¯ = 2(1 + cos ϕ)2 + 2 sin2 ϕ = 2(2 + 2 cos ϕ) = 8 cos2 ϕ/2. det(E − S) This determinant is zero if ϕ = π, i.e. only for a ¯2 axis. In all other cases, Equation (7.4) has a solution, and zero translation can be obtained through a change in origin. Let us therefore consider the operations associated to a ¯2 axis. We recall that a ¯ 2 axis is equivalent to a mirror perpendicular to it, which goes through the inversion center used for the rotoinversion. The rotation angle ϕ is equal ⎛ 0 ⎝ 0 0

to π, and Equation (7.4) becomes: ⎞ 0 0 0 0 ⎠ OO = t. 0 2

This equation has a solution only if t is parallel to axis Oz, the rotoinversion axis, and therefore perpendicular to the mirror.

Chapter 7 – Space groups

135

Let us note this translation t⊥ , and the associated symmetry operation (m, t⊥ ). In this case OO = t⊥ /2. We deduce the following result (Exercise 4.1): The product of a mirror operation and a translation t⊥ , perpendicular to this mirror, is equivalent to a mirror operation without translation provided the mirror is translated by t⊥ /2. The mirror operations which cannot transform into (m, 0) (pure mirrors) through displacement of the mirror are therefore of the form (m, t// ) where t// is parallel to the mirror. We calculate the product of this mirror operation by itself, using Equation (7.3). (m, t// )2 = (m, t// )(m, t// ) = (E, m t// + t// )= (E, 2t// ) which must be a symmetry operation of the crystal, and more precisely a lattice translation since the rotation part is the identity operation. Therefore 2t// must be a crystal lattice vector. We choose in the mirror plane two elementary lattice translations, which we note as a and b. We must have 2t// = ua + vb with u and v integers: u v (7.5) t// = a + b. 2 2 Since the required translations t// are deﬁned modulo the lattice translations, the solutions are restricted to the following cases: (a) t// = a/2 (u = 1 and v = 0): the mirror is called an axial mirror and noted as a, (b) t// = b/2 : the mirror, called axial, is noted b, (c) t// = a/2 + b/2 (u = 1 et v = 1) : the mirror, called diagonal is noted n, (d) t// = 0 : the mirrors without translation, or pure mirrors, are noted m. We chose to call a and b the basis vectors parallel to the mirror, i.e. to consider a mirror parallel to the (a, b) plane. Clearly, the mirror can be parallel to the (a, c) plane, with a translation a/2 (a-type mirror) or c/2 (c mirror), or a/2 + c/2 (n mirror). It can also be parallel to the (b, c) plane with a translation b/2 (b mirror) or c/2 (c mirror) or b/2 + c/2 (n mirror). Tables 7.2 and 7.3 show the symbols used to represent these various mirrors, for two orientations of the projection plane: perpendicular to the mirror for Table 7.2, and parallel to the mirror for Table 7.3. In order to keep the presentation simple, we assumed that the projection plane is parallel to a and b and that, in the case of a monoclinic lattice, c is the basis vector perpendicular to the two others. When the unit cells are multiple, we must also take into account the vector, or vectors, describing the lattice mode, which we note as T . For example,

136

Symmetry and Physical Properties of Crystals Table 7.2: Representation of mirrors perpendicular to the projection plane (a, b)

Nature of the mirror Notation Graphical representation Pure mirror

Translation

m

none

a, b

1/2 along the projection

c

1/2 perpendicular to the projection plane

n

1/2 along the projection + 1/2 perpendicular to the projection plane

Axial mirror

Diagonal translation mirror

Table 7.3: plane (a, b)

Representation of mirrors parallel to the projection

Nature of the mirror Notation Graphical representation

Translation

Pure mirror

m

none

Axial mirror

a, b

1/2 along the arrow

n

1/2 along the arrow

Diagonal translation mirror

for an I lattice, the vector 12 (a + b + c) and, for an F lattice, the three vectors 12 (b + c), 12 (c + a) and 12 (a + b) which complement the (integral) translations ua + vb + wc. Mirrors parallel to these lattice mode vectors, with a glide equal to T /2, are then possible. These mirrors are called diamond mirrors, because they exist in the diamond structure, introduced in Section 7.5.3. Their symbol is d.

7.2.3. Product of a symmetry operation and a translation We return to the cases where a change of origin can change an operation (S(O), t) into (S(O ), 0), whether S is a rotation or a rotoinversion, in order to ﬁnd the rules for performing this change in origin easily. We thus investigate successively the product of a rotation and a translation perpendicular to the rotation axis, of a mirror symmetry and a translation perpendicular to the mirror, and of a rotoinversion and any translation. In all these cases, the result of the product with the translation is just a displacement of the symmetry element implied (rotation axis, mirror or rotoinversion axis).

Chapter 7 – Space groups

137

Product of a rotation and a translation perpendicular to the rotation axis Consider a symmetry operation (S, t⊥ ) where S is a rotation by ϕ = 2π/n about an axis An going through point O, and t⊥ is a translation perpendicular to this axis. Condition (7.2) can be represented geometrically in the plane perpendicular to the rotation axis going through O (Fig. 7.3). We can search for O in this plane, since the position of the origin of rotations along an axis is arbitrary. Let OO be the transform of OO through rotation S. Condition (7.2) shows that O O must be equal to t⊥ . The ﬁgure shows a vector OP equal to O O , hence to t⊥ , as well as parallelogram OPO O . We see that the required point O is the apex of an isosceles triangle with the vector t⊥ drawn from O for its base, and with the rotation angle ϕ for its apical angle. We can thus state the following rule: Operation [S(O), t⊥ ] where S(O) is a rotation by ϕ around an axis going through O, and t⊥ a translation perpendicular to the axis, is equivalent to the pure rotation [S(O ), 0] if point O is on the perpendicular bisector of the segment t⊥ drawn from O and if, from this point, vector t⊥ subtends angle ϕ. O”

t

O

O’

t

P

Figure 7.3: Schematic diagram illustrating Equation (7.2). The new axis of rotation is located at O , on the bissector of OP = t⊥ . Here are two examples of applications. 1.

Consider a crystal with an orthorhombic unit cell, with 2-fold axes parallel to the basis vector c, and choose the origin of the unit cell on one of these 2-fold axes. Figure 7.4a is a projection of the orthorhombic unit cell onto a plane perpendicular to c. Because the crystal is periodic, there is also a 2-fold axis at the other apices of the unit cell. Consider operation [S(O), a], the product of operation S, a rotation by π around the 2-fold axis going through point O, and the lattice translation a perpendicular to the axis. This symmetry operation is equivalent to an operation [S(O ), 0]. According to the above rule, O lies on the perpendicular bisector of segment OA = a, and the angle which OA subtends from O is π. O is therefore the middle of segment OA (Fig. 7.4a). In the same way, performing the product of this rotation by π around the axis going through O and of the translation a + b (or b), we obtain a 2-fold axis located at the center S of rectangle OABC (or at O such that OO = b/2), etc. The set of 2-fold axes present in the unit cell are shown on Figure 7.4b.

2.

Consider a crystal with a tetragonal unit cell featuring 4-fold axes parallel to basis vector c. Figure 7.4c is the projection of this unit cell onto a

138

Symmetry and Physical Properties of Crystals plane perpendicular to c. Let S be the operation rotation by π/2 around the 4-fold axis parallel to c and going through O. Operation [S(O), a] is equivalent to [S(O ), 0] if O is at the center of unit cell OABC because segment OA subtends an angle π/2 from O . Further, a 4-fold axis contains a 2-fold axis which, when combined with the lattice translations, leads to the existence of the 2-fold axes represented on Figure 7.4c. O O’ a

O”

b

C

b

O /2

S

C

O’

a

A

B

(a)

A

(b)

B

(c)

Figure 7.4: (a) Primitive orthorhombic unit cell featuring a 2-fold axis at each lattice node; (b) set of 2-fold axes obtained through the composition of the symmetry operations around these axes with the lattice translations; (c) set of symmetry operations of a tetragonal unit cell of a lattice featuring a 4-fold axis at each lattice node Product of a mirror operation and a translation perpendicular to the mirror The symmetry operation (m, t⊥ ) resulting from the combination of a mirror operation and a translation t⊥ perpendicular to it is equivalent to (m, 0) if the mirror is translated by t⊥ /2. This rule, derived in Section 7.2.2 and in Exercise 4.1, and the previous one, are widely used to determine all the symmetry operations present in a unit cell starting from the generating elements of the space group and the lattice translations. Product of a rotoinversion and a translation We give the results without derivation in order not to make the text too long. The operation product of an inversion (equivalent to a 1¯ axis) and a translation t is equivalent to an inversion without translation if the center is translated by t/2. To determine the change in origin which makes it possible to cancel the trans¯ t) where S ¯ is a rotoinversion associated to a ¯3, ¯4, lation in an operation (S, or ¯6 axis, the translation must be decomposed into its t// and t⊥ components, respectively parallel and perpendicular to the axis. Component t⊥ is canceled by an operation similar to that of Section 7.2.3: point O is replaced by point O located in the plane perpendicular to the axis which goes through O and on the perpendicular bisector of segment OP = t⊥ , such that, from O , OP subtends the angle ϕ − π. Component t// is canceled by submitting O to ¯ ¯ ), 0]. t] = [S(O translation O O = t// /2. We thus obtain [S(O),

Chapter 7 – Space groups

139

7.3. Enumeration of space groups Starting from a given point group G0 G0 = (E, 0) + (S1 , 0) + (S2 , 0) + (S3 , 0) + . . . + (Sm , 0), we want to determine the various space groups Gs which are associated to it, and which can be written as: Gs = (E, 0) + (S1 , t1 ) + (S2 , t2 ) + (S3 , t3 ) + . . . + (Sm , tm ) (modulo T), taking into account the fact that the operations (Si , ti ), where ti is nonzero, are associated to screw axes or to glide mirrors. We recall that all the operations (Si , ti ) here have a common origin. This determination can be performed systematically for all the point groups, starting from the simplest ones and using a few theorems deduced from the isomorphism between the quotient group G/T and the point group G0 to which it is associated. This procedure is tedious, and we will just illustrate the method through an example, that of the space groups deduced from point group mm2. Point group mm2, associated to an orthorhombic unit cell with basis vectors a, b and c, contains the following symmetry operations: rotation by π around an axis which we can assume to be parallel to c for example, and which we note (A, 0), symmetry with respect to a mirror perpendicular to a, which we call (m1 , 0), symmetry with respect to a mirror perpendicular to b, which we note (m2 , 0), and identity (E, 0). G0 = (E, 0) + (A, 0) + (m1 , 0) + (m2 , 0). The mirrors intersect along the 2-fold axis, here parallel to c.

7.3.1. Symmorphic space groups The ﬁrst space group that comes to mind is group Gs , associated directly to point group G0 : Gs = (E, 0) + (A, 0) + (m1 , 0) + (m2 , 0) (modulo T). This means that all the symmetry operations of the crystal are the four operations forming G0 and all their products with lattice translations n = ua +vb + wc. We now choose an axis system Oxyz, parallel to a, b, and c respectively, and take for a unit, along each of these axes, the length of the respective lattice parameter, a, b or c. If an atom in the unit cell has coordinates x, y, z, the presence of the symmetry elements implies the existence of an atom of the same

140

Symmetry and Physical Properties of Crystals

kind at points with coordinates −x, −y, z (operation A, 0), −x, y, z (operation m1 , 0) and x, −y, z (operation m2 , 0). Additionally, there are of course all the positions deduced from the above through the lattice translations, but this goes without saying. Thus the “equivalent positions” of an atom in a general position are deﬁned. The coordinates of these positions are: (x, y, z)

(−x, −y, z)

(−x, y, z)

(x, −y, z).

The space group is noted as Pmm2, with P saying that the lattice is primitive. Consider the cases where the orthorhombic unit cell is a multiple cell. We know it can be base-centered (A, B or C lattice), body-centered (I lattice) or face-centered (F lattice). (a) Body-centered lattice. The crystal lattice features, apart from the translations n = ua + vb + wc which form group T, a lattice mode translation T with coordinates ( 12 , 12 , 12 ). The corresponding space group will be deﬁned by the set of the above operations and of those deduced from them through translation T , so that the new space group is: Gs = (E, 0) + (A, 0) + (m1 , 0) + (m2 , 0) + (E, T ) + (A, T ) + (m1 , T ) + (m2 , T ) (modulo T). The coordinates of equivalent positions are now: (x, y, z)

(x + 1/2, y + 1/2, z + 1/2)

(−x, −y, z)

(−x + 1/2, −y + 1/2, z + 1/2)

(−x, y, z)

(−x + 1/2, y + 1/2, z + 1/2)

(x, −y, z)

(x + 1/2, −y + 1/2, z + 1/2).

This new space group is called Imm2.

(b) Base-centered lattice. For example, in the A lattice, translation T 0, 12 , 12 is added, and the corresponding space group is noted Amm2. The coordinates of equivalent positions will now be: (x, y, z)

(x, y + 1/2, z + 1/2)

(−x, −y, z)

(−x, −y + 1/2, z + 1/2)

(−x, y, z)

(−x, y + 1/2, z + 1/2)

(x, −y, z)

(x, −y + 1/2, z + 1/2).

(c) Face-centered lattice. The F lattice adds translations T 1 0, 12 , 12 , T 2 ( 12 , 0, 12 ), T 3 12 , 12 , 0 . The space group for the F lattice, noted Fmm2, is thus: Gs = (E, 0) + (A, 0) + (m1 , 0) + (m2 , 0) + (E, T 1 ) + (A, T 1 ) + (m1 , T 1 ) + (m2 , T 1 ) + (E, T 2 ) + (A, T 2 ) + (m1 , T 2 ) + (m2 , T 2 ) + (E, T 3 ) + (A, T 3 ) + (m1 , T 3 ) + (m2 , T 3 ) (modulo T)

Chapter 7 – Space groups

141

and the equivalent positions are: (x, y + 1/2, z + 1/2)

(x, y, z)

(−x, −y, z) (−x, −y + 1/2, z + 1/2) (−x, y, z)

(−x, y + 1/2, z + 1/2)

(x, −y, z)

(x, −y + 1/2, z + 1/2)

(x + 1/2, y, z + 1/2)

(x + 1/2, y + 1/2, z)

(−x+ 1/2, −y, z+ 1/2) (−x+ 1/2, −y+ 1/2, z) (−x + 1/2, y, z + 1/2)

(−x + 1/2, y + 1/2, z)

(x + 1/2, −y, z + 1/2)

(x + 1/2, −y + 1/2, z).

This provides the enumeration of the so-called symmorphic space groups, which are the space groups where all the symmetry operations are of the form (S, 0) modulo the lattice translations T for the primitive unit cells, or (S, 0) and (S, T ) modulo T for the multiple unit cells. The number of these space groups for a given crystal system is equal to the number of point groups multiplied by the number of Bravais lattices. We thus obtain a total of 66 symmorphic space groups (Tab. 7.4). Their notation includes a letter which deﬁnes the lattice, followed by the symbol for the point group. Table 7.4: Enumeration of the 66 symmorphic groups, to which 7 supplementary groups must be added

System

Number of point groups

Number of Bravais lattices

Number of space groups

Triclinic

2

1

2

Monoclinic

3

2

6

Orthorhombic

3

4

12

Tetragonal

7

2

14

Rhombohedral

5

1

5

7+5

1

12

5

3

15

Hexagonal Cubic

Seven other groups must be added to these 66 groups, for two diﬀerent reasons. On the one hand, there can be various ways of associating the Bravais lattice translation T to a given point group. This is the case for the basecentered orthorhombic groups, associated to point group mm2, for which it is

142

Symmetry and Physical Properties of Crystals

not equivalent to center the bases parallel or perpendicular to the 2-fold axis: this yields groups Amm2 and Cmm2. On the other hand, there can also be two diﬀerent ways of positioning the symmetry elements with respect to the elementary lattice translations. For example, crystals with point group ¯42m can have their basis vectors parallel either to the mirrors or to the 2-fold axes, and this results in the existence of two diﬀerent space groups, P¯42m and P¯4m2 (the notations are explained in Sect. 7.4). For the same reason, there exist I¯42m and I¯4m2, P312 and P321, P3m1 and P31m, P¯3m1 and P¯31m, P¯6m2 and P¯62m (Exercise 7.1). We thus obtain the 7 supplementary groups (one for the ﬁrst reason, and 6 for the second reason).

7.3.2. Non-symmorphic space groups We again consider point group mm2: G0 = (E, 0) + (A, 0) + (m1 , 0) + (m2 , 0). Primitive groups We replace one or more of the (S, 0) symmetry operations by compatible operations (S, ti ), where the ti are non-zero, i.e. by the operations associated with screw axes or glide mirrors. We ﬁrst replace the pure mirror m2 , perpendicular to basis vector b, by a glide mirror. Symmetry operation (m2 , 0) is thus successively replaced by the symmetry operations (m2 , a/2), (m2 , c/2) and (m2 , a/2+c/2) while retaining (m1 , 0). The symmetry operations have a common origin, chosen on the 2-fold axis where mirrors m1 and m2 intersect. 1.

The group contains, instead of (m2 , 0), operation (m2 , a/2) associated to an a-type mirror. It also contains, by assumption, (m1 , 0), and therefore the product (m2 , a/2)(m1 , 0), calculated using Equation (7.3). This product is equal to (A, a/2), where the 2-fold axis goes through the common origin O. Since translation a/2 is perpendicular to the 2-fold axis, a change in the position of this axis leads to zero translation. Applying the rule of Section 7.2.3 shows that the new axis goes through point O such that OO = a/4 (Fig. 7.5a), since segment OP = a/2 subtends angle π from O . The space group is Gs = (E, 0) + (m1 , 0) + (m2 , a/2) + (A, 0)

(modulo T)

(7.6)

where the indicated operations now do not all have the same origin. Relation (7.6) must be used in connection with Figure 7.5b, which shows the respective positions of the symmetry elements. This group is called Pma2 (group 28 in I.T. A) because we will see, in Section 7.4, that the notation of the space groups in the orthorhombic system is based on the following order for the symmetry elements: ﬁrst the mirror

Chapter 7 – Space groups b

O

m1 O’

a

143

O

C

O’

P A m2

B

(a)

(b)

(c)

(d)

(e)

(f)

Figure 7.5: An example of the determination of space groups deduced from point group mm2. Operation (m2 , 0) is successively replaced by (m2 , a/2), leading to group Pma2 ((a) and (b)), then by (m2 , c/2), leading to space group Pmc21 ((c) and (d)), and ﬁnally by (m2 , a/2 + c/2), leading to space group Pmn21 ((e) and (f)). perpendicular (or the axis parallel) to a, then the mirror perpendicular (or the axis parallel) to b, then the same for c. Figure 7.5b shows the corresponding unit cell OABC, with all the symmetry elements in the unit cell indicated. They are determined by applying the rules of Section 7.2.3 to the products of the operations m1 , m2 and A with the lattice translations. For example the product of (m1 , 0) and the lattice translation a perpendicular to m1 is equivalent to a pure mirror translated by a/2 (rule in Sect. 7.2.3). In the same way, the product of (m2 , a/2) and the lattice translation b perpendicular to m2 yields the same glide mirror translated by b/2. Applying the rule of Section 7.2.3 shows that the combination of the 2-fold axis going through O with a lattice translation n perpendicular to it (here a or b or (a + b)) is equivalent to the existence of a 2-fold axis translated by n/2. Thus there are 2-fold axes going through the points deduced from O through translations a/2, b/2 and (a + b)/2.

144 2.

Symmetry and Physical Properties of Crystals The group contains, instead of (m2 , 0), operation (m2 , c/2) associated to a c mirror. The product (m2 , c/2) (m1 , 0) is equal to (A, c/2), i.e. to a screw axis 21 at the intersection of the mirrors (Fig. 7.5c) and Gs = (E, 0) + (m1 , 0) + (m2 , c/2) + (A, c/2) (modulo T). The space group is noted Pmc21 (group 26, I.T. A) and Figure 7.5d shows all the symmetry elements present in the unit cell.

3.

The group contains, instead of (m2 , 0), operation (m2 , a/2 + c/2) associated with an n mirror. The product operation (m2 , a/2 + c/2)(m1 , 0) is equal to (A, a/2 + c/2), which can be replaced by operation (A, c/2) if the origin of the 2-fold axis is displaced by a/4 (Fig. 7.5e). The space group is Gs = (E, 0) + (m1 , 0) + (m2 , a/2 + c/2) + (A, c/2) (modulo T). It is noted Pmn21 (group n◦ 31, I.T. A) and Figure 7.5f shows all the symmetry elements present in the unit cell.

Other space groups are obtained by substituting glide mirrors for the two mirrors: for example (m1 , b/2) and (m2 , a/2). The product of these two operations is equal to (A, −a/2+b/2), which becomes (A, 0) if the rotation axis is submitted to translation −a/4 + b/4. The group is noted Pba2 (group 32, I.T. A). In the same way, the reader can, as an exercise, consider the various possible combinations of glide mirrors (Exercise 7.3 is an example). This will show that the combination of operations: (m1 , c/2) and (m2 , a/2) leads to group Pca21 (group 29, I.T. A), (m1 , b/2 + c/2) and (m2 , a/2) leads to group Pna21 (group 33, I.T. A), (m1 , c/2) and (m2 , c/2) leads to group Pcc2 (group 27, I.T. A), (m1 , b/2 + c/2) and (m2 , c/2) leads to group Pnc2 (group 30, I.T. A), (m1 , b/2 + c/2) and (m2 , a/2 + c/2) leads to group Pnn2 (group 34, I.T. A). We thus enumerated a total of 10 primitive groups associated to point group mm2. Characterizing each of them involves a schematic drawing indicating the position of the various symmetry elements present in the unit cell. Non-primitive groups The non-primitive space groups can be enumerated starting from each of these 10 primitive groups, by adding the lattice mode translation or translations T , which transform(s) them into a non-primitive lattice. However, the combination of a glide mirror and a translation T can yield a pure mirror translated with respect to the ﬁrst one if translation T contains a component, parallel to the mirror, equal to the glide vector.

Chapter 7 – Space groups

145

Thus consider group Pma2, the symmetry elements of which are represented on Figures 7.5b and 7.6a. In Figure 7.6a, the origin of the unit cell is chosen on a 2-fold axis to conform to the International Tables for Crystallography A (Sect. 7.3.3). Suppose the group is now C-type, meaning that base (a, b) is centered, which adds the lattice translation T = 12 (a + b). The symmetry operation corresponding to this translation is noted ST = (E, 1/2 [a + b]) . The new space group includes the operations of Gs given in Equation (7.6), which must be associated to Figure 7.6a, and the result of combining them with ST . We investigate them in turn. b

a

(a)

(b)

(c)

Figure 7.6: Symmetry elements present in the unit cells of (a) group Pma2; (b) group Pma2 with the (a, b) faces centered, becoming Cmm2; (c) group Cmm2 when the origin is placed on an intersection of two pure mirrors as in I.T. A The composition of (m2 , a/2) with ST is obtained by using relation (7.3), where the rotation or rotoinversion operations are taken to have the same origin. (E, 1/2 [a + b]) (m2 , a/2) = (m2 , [a + b/2]) = (m2 , b/2)

(7.7)

modulo T.

We ﬁnally obtain a glide mirror operation, with a translation b/2 perpendicular to the mirror. It transforms into a pure mirror operation by translating the mirror by b/4 (Fig. 7.6b). Relation (7.7) leads to the remark that combination with a pure translation simply adds this translation to the original translation part. The composition of (m1 , 0) with ST gives (m1 , a/2 + b/2). The translation part has two components: a/2, perpendicular to the mirror, which can be canceled by translating the mirror by a/4, and b/2, parallel to the mirror, which turns it into a glide mirror. Combining (A, 0) with ST displaces the 2-fold axis by 14 (a + b). All the symmetry elements present in the unit cell are represented on Figure 7.6b. We see that there are pure mirrors perpendicular to a and b. The space group is Cmm2. Figure 7.6c shows the unit cell, taking for the origin the intersection of mirrors as in volume A of the International Tables for Crystallography.

146

Symmetry and Physical Properties of Crystals

In contrast, if a lattice translation T = 12 (b + c) is added to group Pma2, the lattice becomes base-centered A, and we obtain group Ama2, the symmetry elements of which are shown on Figure 7.7. b

a

Figure 7.7: Symmetry elements of space group Ama2 The non-primitive space groups associated to point group mm2 are thus fewer than the primitive groups. In International Tables A, the following groups are found: Cmm2, Cmc21 , Ccc2, Amm2, Abm2, Ama2, Aba2, and Fmm2. The aim of this section was to show one procedure for the enumeration of space groups. Their complete enumeration is beyond the scope of this book. There are 230 crystallographic space groups, perfectly described in volume A of International Tables for Crystallography, which is presented in the following section.

7.3.3. International Tables for Crystallography The 230 space groups are cataloged in volume A of the International Tables for Crystallography (I.T. A) which, for each group, provide lots of information, as shown on the two pages reproduced on Figures 7.8 a and b, dedicated to space group P4/n, numbered 85. The ﬁrst of theses pages is reproduced on Figure 7.8a. The ﬁrst line indicates the name of the space group in the Hermann-Mauguin 3 ), then the associated notation (P4/n), then in the Schönﬂies notation (C4h point group (4/m), and ﬁnally the associated crystal lattice (tetragonal). Since the lattice is primitive, the orders of the space group and the point group are equal, in this case to 8. The 8 symmetry operations of the space group are listed under “Symmetry operations”, where each operation is numbered and its nature and position described. For example operation (6), noted n 12 , 12 , 0 x, y, 0, is the symmetry operation “mirror with diagonal translation n”, the glide component of which is the vector 12 , 12 , 0 , with the position of the mirror being given by its equation z = 0 or (x, y, 0). The left-hand ﬁgure is the projection onto a plane perpendicular to the highestorder axis (here the 4-fold axis) of all the symmetry elements present in the unit cell. The basis vectors a and b are oriented as on the earlier ﬁgures (7.5 to 7.7). The symbols used for this representation were introduced in Tables 7.1 to 7.3.

Chapter 7 – Space groups

147

Figure 7.8a: Reproduction of a page of volume A of the International Tables for Crystallography: ﬁrst page describing group P4/n (© IUCr, with permission) The origin of the chosen unit cell is indicated under the ﬁgures. Here it is taken on the center of inversion for the ¯4 axis, and this is the ﬁrst choice of the International Tables A. For this group, the Tables also oﬀer another version, not reproduced here, where the origin of the unit cell is chosen on a center of symmetry. The right-hand ﬁgure indicates the general positions of the atoms, the signs + and − standing for coordinates + z and − z respectively. The circles with a comma are the images of the circles without comma through one of the improper symmetry operations of the group (mirror, inversion or rotoinversion). Page 2 (Fig. 7.8b) ﬁrst presents a choice of generating elements for the space group, then the various possible positions for an atom (indexed through a letter, called the Wyckoﬀ symbol), starting with the general position, for which the coordinates x, y, z are general. The following positions are special positions, because they are located on one or several symmetry elements. For each position, the table gives the coordinates of the equivalent positions (modulo the lattice translations) through the symmetry operations of the group. For the general position, the atoms in positions equivalent through the symmetry operations are numbered from (1) to (n) where n is the order of the group.

148

Symmetry and Physical Properties of Crystals

Figure 7.8b: Reproduction of a page of volume A of the International Tables for Crystallography: the second page describing group P4/n (© IUCr, with permission) The atom in position (k) deduces from atom in position (1) through the symmetry operation indexed as (k) on the ﬁrst page. For example, in the space group P4/n described, atom (3) deduces from atom (1) through operation (3), a rotation by π/2 around the 4-fold axis which goes through the point with coordinates x = 0, y = 12 . For each position, the table starts out by indicating its multiplicity (number of equivalent positions), then its Wyckoﬀ symbol (a letter given in alphabetical order, starting with the last position, the one with lowest multiplicity), then the local symmetry of this particular site, and ﬁnally the coordinates of the equivalent atomic positions. The local symmetry of a site in a special position deduces from the symmetry elements going through the site. The set of the symmetry operations associated to these symmetry elements which intersect

Chapter 7 – Space groups

149

on the site form a point group which is a subgroup of the point group of the crystal. The asymmetric unit, indicated on page 1, is deﬁned in a general way as a part of space such that, if it is submitted to all the symmetry elements of the space group, all of space is occupied. It is therefore bounded by planes. However, for a given crystal structure, the asymmetric unit is deﬁned by a group of atoms such that, when complemented by their images through all the symmetry operations of the space group, the motif (or pattern) of the crystal unit cell is retrieved. We note that the set of atoms in the motif of a crystal correspond to a multiple of the chemical formula of the material, while this is not necessarily the case for the atoms in the asymmetric unit. For example, the motif of the unit cell of quartz (chemical formula SiO2 , space group P31 21) contains three SiO2 groups, while the asymmetric unit consists of one Si atom and one O atom. Since the oxygen atom is in a general position with multiplicity 6, there are 6 oxygen atoms in the motif while the Si atoms are in a special position (on a 2-fold axis) with multiplicity 6/2 = 3, hence 3 silicon atoms in the motif. Starting with one Si atom and one O atom, we retrieve the set Si3 O6 , i.e. a motif of three SiO2 groups.

7.4. Nomenclature The Hermann-Mauguin space group notation starts with a letter indicating the nature of the Bravais lattice (P for primitive, A, B or C for base-centered, I for body-centered, and F for face-centered). It then refers directly to the notation of the point group which is associated to it (the notation is given in Chap. 5), making explicit the nature of the axes and mirrors involved in the notation for the point group. For example, if an n-fold axis is a screw axis, we add to the n involved in the point group notation a subscript p indicating that the translation is a fraction p/n of the basis vector parallel to the axis (Tab. 7.1). If one of the mirrors is a glide mirror, the letter m is replaced by a, b, c or n depending on the nature of the translation (Tab. 7.2). When the notation for the point group includes several identical signs, or involves an ambiguity, the following rules are applied, with the understanding that the quoted directions deﬁne, when the subject is an axis, its direction, and, for a mirror, the direction perpendicular to it. Orthorhombic system: the order is a, b, c. Example: group Cmc21 . The unit cell has its (a, b) bases centered. The point group is mm2. There are pure mirrors perpendicular to a, glide mirrors (translation c/2) perpendicular to b, and screw axes parallel to c (translation c/2). Tetragonal system: the ﬁrst sign refers to the 4 or ¯4 axis, which is always parallel to c, the second to the directions a and b, equivalent to each other, and the third to the bisectors of these directions in the (a, b) plane.

150

Symmetry and Physical Properties of Crystals Example: P¯ 42m is a space group with a primitive unit cell, with point group ¯42m. The ¯4 axis is parallel to c, there are 2-fold axes parallel to a and b, and pure mirrors at 45◦ to a and b. In group P¯4m2, the mirrors are parallel to a and b and the 2-fold axes are at 45◦ to a and b (Exercise 7.1). Hexagonal system: the ﬁrst sign refers to the 6-fold axis, parallel to c, the second to the directions of vectors a and b, and the third to the directions perpendicular to a and b. Example: P63 cm is a space group with a primitive unit cell, with point group 6mm; the 6-fold axis, parallel to c, is a screw axis (translation c/2); there are glide mirrors (glide c/2) perpendicular to a and b and pure mirrors parallel to a and b (since they are perpendicular to the normals to a and b). We now understand, on the basis of these examples, the rationale for the redundancy in the notation for some point groups. For example, in point group 6mm, the notation 6m is suﬃcient as a descriptor, since the generating elements of the group are the 6-fold axis and a mirror which contains it: the presence of these two generators leads to the existence of 6 mirrors enclosing angles of 30◦ with one another. However, these mirrors form two distinct families with respect to the symmetry operations of the space group. This leads to the existence of two diﬀerent space groups, P63 mc and P63 cm. Special case of the hexagonal lattices with rhombohedral point group: we recall (Sect. 6.3.3) that a crystal with rhombohedral point group (3, ¯3, 32, 3m or ¯3m) can have a rhombohedral lattice (noted R) or a hexagonal lattice (noted P). The rule for the hexagonal lattices applies to those with a hexagonal lattice, but with a 1 inserted where there is no symmetry element. Example of the group P31 21: the unit cell is hexagonal, the point group is 32, the 3-fold axis, parallel to c, is a screw axis (translation c/3), the 2-fold axes are parallel to a and b, and there is no 2-fold axis perpendicular to a and b. In contrast, for group P31 12, the 2-fold axes are perpendicular to a and b. Cubic system: same order as for the point group, viz. directions of the cube sides, then directions of the major diagonals of the cube, then directions of the face diagonals. First example: Pn¯3: primitive unit cell, point group m¯3, glide mirrors perpendicular to the cube edges (translation 12 (b + c) for the mirror perpendicular to a), 3-fold axes parallel to the major diagonals of the cube, and center of symmetry. ¯ Second example: Fd¯3m: face-centered cubic unit cell, point group m3m, diamond mirrors (see Sect. 7.2.2) perpendicular to the cube sides (translation 14 (b + c) for the mirror perpendicular to a), 3-fold axes parallel to

Chapter 7 – Space groups

151

the major diagonals of the cube and center of symmetry, pure mirrors perpendicular to the face diagonals. This is the space group of diamond and silicon crystals (see Sect. 7.5.3).

7.5. Examples: space groups of some structures 7.5.1. TiO2 -type structure (rutile) This structure2 is represented in a perspective view on Figure 8.4b. The unit cell is tetragonal primitive. The positions of the atoms in the unit cell are: Ti atoms : 0, 0, 0 and 12 , 12 , 12 ; O atoms:

u, u, 0;

1 2

+ u,

1 2

− u, 12 ;

1 2

− u,

1 2

+ u, 12 ;

−u, −u, 0.

The projection onto plane (a, b), with the heights z indicated, of the atom positions in two neighboring unit cells is shown on Figure 7.9a. The Ti atoms are shown as full circles and the O atoms as empty circles. This evidences a 42 axis which projects at A, glide mirrors (n mirrors) perpendicular to the sides a and b, with glides respectively 12 (b + c) and 12 (a + c), and pure mirrors parallel to the diagonals of the square. There is also a mirror parallel to the plane of the ﬁgure at height 0 (and another one at height 12 ). The point group is thus 4/m mm and the space group is P 42 /m nm. Since the point group is centrosymmetric, so is the space group. A center of symmetry projecting at A, with height 0, is evidenced. Figure 7.9b shows the axes and mirrors perpendicular to the projection plane. The 42 axis contains a 2-fold axis, and the products of the symmetry operations associated to this 2-fold axis with the lattice translations produce 2-fold axes at the apices and at the center of square (a, b). The centers of symmetry, represented by empty circles as usual, are also shown. Figure 7.9c shows all the symmetry elements present in the unit cell; this ﬁgure is excerpted from International Tables volume A (group 136). We note that the asymmetric unit here consists of one Ti atom and just one O atom, while the motif, outlined in dotted lines on Figure 7.9a, contains two TiO2 groups. The order of the point group is 16. It is equal to that of the space group since the unit cell is primitive. There are therefore 16 equivalent atoms in general positions. The oxygen atom is in a special position, at the intersection of two pure mirrors, hence on a site with multiplicity 16/4 = 4 while the Ti atom is at the intersection of 3 pure mirrors, thus on a site with multiplicity 16/8 = 2. Many crystals have this structure. Examples are CoF2 , MnF2 , CrO2 , PbO2 . The values of a, c and u vary from compound to compound.

2. TiO2 also exists under two other forms: anatase (tetragonal, I4/a md) and brookite (orthorhombic, Pbca).

152

Symmetry and Physical Properties of Crystals 0

b 0

0 0

0 0

½

a

½

A

½ ½

½ 0

0

Ti O

A

½ 0

0

0 0

0

(a)

(b) ¼

– –1 : 0 4:¼

¼

¼

¼

– 1 –:0 4:¼

– –1 : 0 4:¼

¼

¼

¼

– 1 –:0 4:¼ ¼

(c)

Figure 7.9: Structure of TiO2 . (a) Projection of the atoms onto plane (a, b), with the heights (z-coordinate) indicated. The Ti atoms are full circles and the O atoms empty circles. The dotted line surrounds the atoms which form the crystal motif. (b) Projection onto the same plane of the axes and mirrors present in the unit cell which are perpendicular to the plane. (c) Projection of all the symmetry elements present in the unit cell. Reproduction of a ﬁgure from volume A of the International Tables for Crystallography (© IUCr, with permission).

7.5.2. Metals with close-packed hexagonal structure This is the case for example of Zn, Na, Be, Mg, Cr. In this structure, which will be described in Chapter 8, the unit cell is hexagonal, with an atom at each of its vertices and another atom at position ( 23 , 13 , 12 ) as shown on Figure 7.10a, a projection of the atomic positions onto the base plane (a, b) indicating their coordinate parallel to c. Several contiguous unit cells were drawn in order to make the determination of the symmetry elements in this structure easier. By looking at the atom positions, we ascertain the presence of a 63 axis projecting at point A, a pure mirror with trace MN and two other mirrors of the same family (enclosing 60◦ angles between one another) going through A. We also distinguish a glide mirror with translation c/2, with trace uu (and two other mirrors of the same family going through A). Further, the plane of the ﬁgure (as well as the plane parallel to it at height 12 ) is a symmetry plane, hence

Chapter 7 – Space groups

M

153

0

0

½

u a 0

center of symetry at height ¼

½

b A

0

0

0

b

0

u’

½

a

½ 0

0

N

(a)

(b)

¼

¼

¼ ¼

¼

¼ ¼

¼ ¼

¼ ¼

¼

¼

¼

¼

¼ ¼

¼

¼

¼ ¼

¼

¼

¼

¼

¼

¼

¼ ¼

¼ ¼

¼ ¼

¼ ¼

¼ ¼

¼ ¼

¼ ¼

(c)

Figure 7.10: Close-packed hexagonal structure: (a) projection of the atomic positions, with the heights indicated, of four adjacent unit cells onto a plane perpendicular to c; (b) projection of some of the symmetry elements present in the unit cell; (c) projection of all the symmetry elements present in the unit cell, reproduced from I.T. A (group 194). The origin of the unit cell is at a center of symmetry located on the 63 axis. a pure mirror. We deduce that the space group is P 63 /m mc (group 194 in I.T. A). The point group is 6/m mm, which has a center of symmetry. There is a center of symmetry at height 14 , which projects at A. Figure 7.10b shows a single unit cell and the symmetry elements we just determined. Figure 7.10c shows all the symmetry elements in the unit cell, as found in International Tables volume A. We note, however, that, in International Tables, the origin of the unit cell is located on a center of symmetry which, on Figure 7.10a, projects at A and has height 14 . This explains why the mirror, parallel to the plane of the ﬁgure, which was at height 0 (with another one at

154

Symmetry and Physical Properties of Crystals

height 12 ) on Figure 7.10b, is at height 14 on Figure 7.10c, while the center of symmetry is noted with no further indication on Figure 7.10c since it is in the projection plane.

7.5.3. Structure of diamond The structure of diamond is shown on Figure 8.6 in a perspective view. This is also the structure of silicon and germanium. The unit cell is face-centered cubic and the projection of the carbon atoms onto the plane perpendicular to one of the sides of the cubic cell, the (a, b) plane for example, is represented, with height indications, on Figure 7.11a. The motif (or pattern) consists of two atoms (surrounded by a dotted line), with coordinates respectively (0, 0, 0) and ( 14 , 14 , 14 ). This structure features 3-fold axes along the major diagonals of the cubic unit cell. 0

0

½ ¾

¼

b ½ ¼

0,½ ¼,¾

0

0

0,½

½

0,½

0,½

3⁄8

1⁄8

1⁄8

3⁄8

¾

½

0

a

(a)

(b)

(c)

Figure 7.11: Structure of diamond, with face-centered cubic unit cell: (a) projection of the atom positions, with the heights indicated, onto plane (a, b); (b) position of the symmetry axes parallel to c; (c) projection of the mirrors perpendicular to the (a, b) plane Figure 7.11b shows the projection onto the (a, b) plane of the positions of the symmetry axes perpendicular to this plane. They are 41 , 43 and ¯4 axes. For the ¯4 axes, the height of the point used for inversion is indicated. In order not to clutter the ﬁgure, they are shown only in the upper left quadrant, because the ﬁgure is identical in all four quadrants. In the same way, the position and height of the centers of symmetry are shown only in the upper right quadrant. Figure 7.11c shows the mirrors perpendicular to the plane of the ﬁgure. The mirrors parallel to the cube faces are the glide mirrors with translation 14 (a + c) or 14 (a − c) for the mirrors perpendicular to b, and with translation 14 (b + c) or 14 (b − c) for the mirrors perpendicular to a. The two possibilities are distinguished by an arrow indicating the direction of the component of the translation vector along the projection plane, assuming the component perpendicular to the projection plane is positive. For example, if the translation vector is 14 (a + c), the arrow will be in the direction of a; if it is 14 (a − c), the arrow will be along vector −a, since the sign of the translation vector can be changed: if the translation vector is v to go from atom A to

Chapter 7 – Space groups

155

atom B, it is −v to go from atom B to atom A. These glide mirrors, for which the translation vector is a quarter of a lattice vector deﬁned by vectors a, b and c but half of a lattice mode vector T characterizing a multiple unit cell, are called diamond mirrors and noted d (see Sect. 7.2.2). The diagonal mirrors, perpendicular to the face diagonals, are pure mirrors. According to the rules stated in Section 7.4 (the ﬁrst symbol shows the nature of the mirrors perpendicular to the cube sides, the second symbol indicates the 3- or ¯3-fold axis, and the last symbol indicates the nature of the diagonal mirrors), the space group of the diamond structure is noted Fd¯3m.

7.6. Exercises Exercise 7.1 1.

(a) Consider point group ¯42m. Using a stereographic projection onto a plane normal to the ¯4 axis, show that the generating elements of this group can be either the ¯4 axis and a mirror parallel to this axis, or the ¯4 axis and a 2-fold axis perpendicular to this axis. (b) A crystal with this point group has a tetragonal lattice. Comparing the stereographic projections of the point groups of this crystal and its lattice, show that the basis vectors a and b of this lattice can be parallel either to the 2-fold axes, or to the mirrors. This leads to space groups P¯42m and P¯4m2 respectively. Determine, for each of these space groups, the equivalent positions for the general position x, y, z, and all the symmetry elements in the unit cell. Note that the ¯4 axis is at the intersection of the mirrors, and that the 2-fold axes intersect this ¯4 axis. Choose as the origin of the unit cell the point common to the various symmetry elements.

2.

We consider a crystal with point group 3m, and with a hexagonal lattice. (a) By comparing the point group of the crystal and that of the lattice, show that the three mirrors can be either parallel or perpendicular to the basis vectors a and b. (b) Two diﬀerent space groups are thus deﬁned, P31m and P3m1. Display, through a projection onto a plane perpendicular to the 3-fold axis, all the symmetry elements in the unit cell. (c) Why does the same approach fail to apply if the lattice is rhombohedral (space group R3m)?

Exercise 7.2 1.

Consider space group P4. Indicate all the symmetry elements present in the unit cell through a projection onto a plane perpendicular to the 4-fold axis.

156 2.

Symmetry and Physical Properties of Crystals The space group I4 is obtained by adding translation 12 (a + b + c) to the symmetry operations of group P4. Indicate all the symmetry elements present in the unit cell using a projection onto a plane perpendicular to the 4-fold axis.

Exercise 7.3 Determine the primitive space group deriving from point group mm2 and containing operations (m1 , c/2) and (m2 , a/2) where m1 is the symmetry operation associated to mirror M1 , perpendicular to a, and m2 the one associated to mirror M2 , perpendicular to b. Give its notation and the arrangement of the symmetry elements in the unit cell.

Investigation of some structures The following exercises deal with some crystal structures in the following way. We give the crystal system of the compound, and the position of the atoms in the unit cell. You are asked to determine the corresponding space group. This approach provides a better understanding of the notion of space group, and it is thus well suited to this book. We must however realize that this is not the approach used by a scientist who wants to determine the structure of a given crystal. The researcher starts out from an experimental result: the X-ray diﬀraction diagram given by this crystal. The accurate investigation of this diagram provides information on the space group of the crystal before the positions of the atoms in the unit cell are known. Exercise 7.4: structure of neptunium (Np) Between 278◦ C and 570◦ C, the crystal lattice of neptunium is tetragonal and the Np atoms are at the following positions: 0, 0, 0

1 1 2, 2,

1 2,

0

0, u

0, 12 , u ¯

1.

Determine the Bravais lattice.

2.

What is the local symmetry of each of the Np atoms? Give the corresponding point group for each of the sites, and deduce the group of which these two point groups are subgroups. This yields the point group of the crystal.

3.

Determine the nature of all the symmetry elements which make it possible to determine the space group. Indicate the space group.

Exercise 7.5: structure of NiAs Nickel arsenide, NiAs, crystallizes in the hexagonal system and the atom positions are: Ni As

0, 0, 0 1 2 3, 3, u

and and

0, 0, 12 , 2 1 1 3, 3, u + 2.

Chapter 7 – Space groups

157

1.

Draw a diagram, with the heights speciﬁed, of the atomic positions projected onto the plane perpendicular to c.

2.

Determine the symmetry elements present in the unit cell, and deduce the space group of the crystal.

3.

What is the symmetry of the Ni and As sites?

Exercise 7.6: structure of FeOCl Iron oxychloride FeOCl crystallizes in the orthorhombic system, and the atom positions are: Fe

0, 12 , u

and

Cl O

0, 0, v 0, 0, v

and and

1 2, 1 2, 1 2,

0, −u 1 2, 1 2,

−v −v

1.

Determine the Bravais lattice.

2.

Draw a diagram of the projection of the atoms onto a plane perpendicular to c, with the heights speciﬁed.

3.

Determine the symmetry elements present in the unit cell and the space group of this crystal.

4.

Give the number of equivalent positions for the general position and the coordinates of these positions.

158

Symmetry and Physical Properties of Crystals

Complement 7C. Structure determination: outline Solving a crystal structure means determining on one hand the geometry of the unit cell, and on the other hand the contents of the unit cell. The geometry involves the lengths and relative orientations of the sides of the unit cell that adequately describes the crystal symmetry. The contents of the unit cell involves the nature of the various atoms or ions, their average positions, and their thermal oscillations. The overwhelming majority of crystal structure determination work is based on the diﬀraction (coherent elastic scattering) of radiation, chieﬂy X-rays but in some cases neutrons. The replication of the unit cell inherent in crystal periodicity then allows ﬁnding the geometric characteristics and contents of the unit cell, whereas this would not be possible for a single unit cell. As shown by Bragg’s law (Sect. 3.2.3), the useful radiations must have wavelength smaller than the interatomic distances, hence the predominant use of X-rays. Neutron and electron diﬀraction, as discussed in Complement 4C, are also used, but to a much lesser extent. The frequency associated for example with X-rays of wavelength 0.05 nm (0.5 Å) is ν = c/λ = 3 × 108 /5 × 10−11 = 6×1018 Hz – far above the tracking possibilities of any instrument. As a result, only the intensity of the X-rays, but never their amplitude and phase, can be detected. Two sets of information must be collected. On the one hand, the geometrical conditions for coherent elastic scattering (diﬀraction) to occur, and on the other hand the eﬃciency of diﬀraction under this condition. The most convenient description of the geometrical condition for an incident wave, with wave-vector k0 , to be diﬀracted into a wave with wave-vector k is that the diﬀerence in wave-vector k − k0 be equal to a reciprocal lattice vector h∗ of the crystal, as introduced in Section 3.2.1 k − k0 = h∗ = ha∗ + kb∗ + lc∗ with a∗ , b∗ and c∗ the basis vectors of the reciprocal lattice and h, k and l integers. The geometrical information thus consists in the orientations and norms of the reciprocal lattice (Sect. 3.2) vectors h∗ , which we recall are vectors in reciprocal (or wave-vector) space. Each of them is associated with a Bragg reﬂection hkl, another name for the coherent elastic diﬀraction process with scattering vector h∗ . Another approach to diﬀraction by crystals consists in noting that, as is the case for visible light, the diﬀraction pattern is the representation of the modulus squared of the diﬀracted amplitude. The latter is the Fourier transform of the quantity which describes the interaction with matter. In the X-ray case, this is the electronic density ρe (r), the number of electrons per unit volume. If the crystal is supposed to be perfectly periodic, the (spatial) Fourier transform is non-zero only for discrete values of the scattering vector k − k0 , just as the

Chapter 7 – Space groups

159

(temporal) Fourier transform of a sound wave (periodic in time) only includes the fundamental frequency and its harmonics. This leads to the reciprocal lattice nodes h∗ = ha∗ +kb∗ +lc∗ shown above and introduced in Section 3.2.1. Each node of the reciprocal lattice, i.e. each vector h∗ , is characterized quantitatively in terms of the integrated reﬂectivity of the Bragg reﬂection Rhkl , the ratio of the area under a curve of diﬀracted power Pd versus crystal angle (rocking curve) over the intensity incident on the crystal: this quantity is signiﬁcant because it is independent of the divergence of the incident beam (Fig. 7C.1). The expression is discussed, without derivation, in the text below, which can be skipped on ﬁrst reading. Slit

Detector

Pd

Source Io

I 2 B

Crystal

(a)

(b)

Figure 7C.1: (a) A rotating crystal diﬀraction measurement on a single crystal. The diﬀracted beam is collected by a detector set at angle 2θB with respect to the incident beam, with θB the Bragg angle. (b) The variation of the diﬀracted power P d with the angle of the crystal, Ω, is the rocking curve. The integral under this curve, scaled with the power P 0 of the incident beam, is the integrated reﬂectivity.

Integrated reﬂectivity for X-rays under the kinematical approximation. Structure factor, Lorentz and polarization factors, Debye-Waller factor The expression for the integrated reﬂectivity can be shown to be Rhkl = λ3 V LP |ρhkl |2 where λ is the wavelength of the radiation used, V the volume of the crystal, L is the Lorentz factor, which depends only on the scattering angle and on the diﬀraction technique used (it is tabulated for example in International Tables for Crystallography, volume C), and P is the polarization factor, which depends only on the scattering angle and on the polarization of the incident beam (it is also tabulated in International Tables for Crystallography, volume C). The central quantity ρhkl is the hkl Fourier component of the scattering length density for the probe used. In the X-ray case, where the scattering is due to the electrons, ρhkl = rc ρe,hkl where rc is the length characterizing diﬀraction by a

160

Symmetry and Physical Properties of Crystals

single free electron and is called the classical electron radius, rc = 2.8×10−15 m and ρe,hkl the Fourier coeﬃcient hkl of the electron density ρe (r) in the crystal. Alternatively, we can write ρe,hkl = Fhkl /Vc , where Fhkl is called the structure factor of the Bragg reﬂection used, and Vc the unit cell volume. It is convenient to include in the expression for the structure factor the eﬀect of thermal vibrations of the atoms or ions through the so-called Debye-Waller factor. Then the structure factor can be written as fj exp[i(hxj + kyj + lzj )] exp{−Wj } Fhkl = j

or Fhkl =

fj exp[i(h∗ · rj )] exp{−Wj }.

j

In this expression, the sum is over all the atoms, indexed by subscript j, in the unit cell; fj is the atomic scattering factor (a function of the norm ||h∗ || of the scattering vector, at least in the approximation where the electron density in the atom has spherical symmetry), rj is the average position vector of the atom; exp{−Wj } is the Debye-Waller factor describing the vibration eﬀect; it reduces the scattering more heavily for those atoms which vibrate strongly, as well as for large scattering vectors. It is important to note that the experimentally measured quantity Rhkl is directly related to |ρhkl |2 and not to ρhkl . If ρhkl could be directly measured, determining the structure would be a trivial matter, since the electron density ρe (r) could then be reconstructed from its Fourier components. Actually the phase information is missing, and this is known as the phase problem in crystallography. Elaborate strategies, the discussion of which is beyond the scope of this complement, have been developed to obviate this problem. Structure determination is a largely computer-automated process. It can be performed with single crystal samples or with powders, where the sample consists of many tiny crystals, oriented at random. Powder diﬀraction, aided by computer ﬁles containing the results from a vast number of phases, is also a valuable tool for material identiﬁcation in industry or geology. More and more elaborate structures, involving larger and larger unit cells and more and more atoms in the unit cell, are determined routinely. A special case is that of materials of biological interest, where both the challenge and the eﬀorts are big, and where outstanding results in terms of basic science as well as for applications in medicine are obtained.

Chapter 7 – Space groups

161

Further reading A. Authier, The Reciprocal Lattice, International Union of Crystallography, Teaching Pamphlets (1981) C.A Taylor, A Non-mathematical Introduction to X-ray Crystallography, International Union of Crystallography, Teaching Pamphlets (2001); http://www.iucr.org/ data/assets/pdf ﬁle/0008/3050/1.pdf J.P. Glusker, Elementary X-ray Diﬀraction for Biologists, International Union of Crystallography, Teaching Pamphlets (2001); http://www.iucr.org/ data/assets/pdf ﬁle/0008/14399/15.pdf J.P. Glusker, K.N. Trueblood, Crystal Structure Analysis: A Primer (Oxford University Press, 1985)

162

Symmetry and Physical Properties of Crystals

References [1] Th. Hahn (ed.), International Tables for Crystallography, vol. A, Spacegroup Symmetry, 5th edn. (Kluwer Academic Publishers, Dordrecht, 2005)

Chapter 8

Chemical bonds and crystal structures This chapter introduces the various types of chemical bonds, and discusses how the nature of the bonds gives an insight into some crystal structures.

8.1. Introduction The periodic structure of crystals was ﬁrst evidenced by X-ray diﬀraction. This technique makes it possible to accurately determine not only the triple periodicity of the atomic arrangement, i.e. the crystal lattice, but also the positions of the individual atoms in the crystal motif. One may ask whether we can explain why one atomic arrangement rather than another one is obtained. This cannot be done in a systematic way. However, some rules emerge, and make it possible in many cases, not actually to predict the crystal structure, but rather, as we will see, to interpret the structure once it is determined. A crystal exists due to the cohesion between atoms, i.e. thanks to the existence of interatomic forces. The crystal structure is determined by the balance between the various interatomic forces. In order to understand the rationale for the various crystal structures, we therefore must start out by investigating these forces, i.e. the nature of chemical bonding in crystals and the special properties of each of these forces. Whatever the nature of the forces, one general rule applies: the atoms arrange in the most compact (or close-packed) way possible consistent with their size and the special requirements due to the nature of the force. The distance between two atoms in a solid results from the balance between the attractive and repulsive forces between these two atoms. The physical nature of the attractive force depends on the solid. It can be electrostatic as in ionic solids, or it can be a covalent binding force, or a Van der Waals force, or. . . Its variation as a function of the distance between the two atoms depends on the nature of these forces. In contrast, the repulsive force, due to the electrostatic repulsion between electrons and to Pauli’s “exclusion principle”,

© Springer Science+Business Media Dordrecht 2014 C. Malgrange et al., Symmetry and Physical Properties of Crystals, DOI 10.1007/978-94-017-8993-6_8

163

164

Symmetry and Physical Properties of Crystals

Energy

which forbids two electrons from being in the same quantum state, may in all cases be approximated by a 1/r 11 or 1/r 12 or exp(−r/ρ) function, where ρ is a characteristic radius. For all types of chemical bonds, the total potential energy looks like the curve shown on Figure 8.1. It has a minimum for a value r0 of r which is the equilibrium position. Since the repulsive energy varies, in all cases, much faster than the attractive energy, its contribution to the total energy at equilibrium (r = r0 ), noted U (r0 ), is small with respect to the attractive energy Eatt (r0 ). We may therefore obtain a fair order of magnitude of the total energy at equilibrium by considering only the attractive energy.

Repulsive energy

0

U(r0) Eatt(r0) Attractive energy 0

1

2

3

4

5

6

r/r0

Figure 8.1: Potential energy between two atoms as a function of their distance, expressed in units of the equilibrium distance r 0 of these two atoms (thick line) In this chapter, we describe the main bonding forces. For each of them, we ﬁrst show the properties of the corresponding arrangements (such as a deﬁnite number of ﬁrst neighbors, or not; well-deﬁned bond directions, or not. . . ). Then we indicate the order of magnitude of the bonding energy. We recall that the bonding energy of two atoms forming a molecule is the diﬀerence in energy between the isolated atoms (i.e. when they are located at inﬁnite distance from each other) and the atoms gathered into a molecule. In a general way, the bonding energy, also called cohesive energy, of a group of atoms forming a molecule or forming a crystal is the diﬀerence in energy between these atoms when isolated and the atoms in the form of the molecule or crystal. Finally, we give for each bond type a few examples of simple structures involving this type of force. We will mostly restrict this description to crystals containing one or two types of atoms.

Chapter 8 – Chemical bonds and crystal structures

165

8.2. Ionic bonds 8.2.1. Nature and properties An ion is an atom which lost or gained electrons, so that its outermost electronic shell is complete. Its electronic structure is then usually that of a rare gas. Example: the Na+ and Cl− ions. Their electronic conﬁguration, together with that of the non-ionized atoms, is shown in Table 8.1. Table 8.1: and ions

Electronic conﬁguration of sodium and chlorine atoms

Electronic state → Element or ion

1s

2s

2p

3s

Na

2

2

6

1

Na+

2

2

6

Cl

2

2

6

2

5

Cl−

2

2

6

2

6

3p

Ionic crystals are made up of positive and negative ions, and the Coulomb interaction is dominant. Because the crystal is neutral, charge compensation must occur, on the smallest scale possible, which leads to an alternation of positive and negative ions. Each ion is attracted by its nearest neighbors and repelled by its second neighbors. X-ray diﬀraction allows to determine accurately not only the positions of the centers of the atoms and thus their distance, but also the distribution ρ(r) of the electronic charge density. The distribution obtained, for example along the axis connecting the Na+ and the Cl− ions, in a crystal of NaCl is shown on Figure 8.2b, deduced from Figure 8.2a. We see that ρ(r) practically goes to zero between the ions (the minimum is less than one thousandth of the maximum density at the center of the ions). This justiﬁes the approach below, where the electrostatic interaction between Na+ and Cl− is treated as that of +q and −q point charges (where q is the electron charge), localized at the center of the ions. In fact, the measurement shown on Figure 8.2 can be performed on many ionic crystals, which are diﬀerent combinations of ions. The results of these accurate measurements lead to the following rule: to a rather good approximation, each species can be described as a “hard sphere” (meaning that it does not deform when it comes to contact), with a well-deﬁned radius called the ionic radius.

166

Symmetry and Physical Properties of Crystals

Electron density [e– Å–3]

200

Cl − 150

100

Na+ 50

0 0

(a)

0.4

0.8

1.2

1.6

2

2.4

2.8

Distance [Å] (b)

Figure 8.2: Electron density in a crystal of NaCl in the (hk0) plane: (a) iso-electron-density curves, after G. Schoknecht [1] (reproduced by kind permission of Verlag der Zeitschrift für Naturforschung, Tübingen, Germany); (b) variation in the electron density along the line connecting a Na+ ion to its nearest neighbor Cl− , as deduced from (a). The distance between the Na+ and Cl− ions is 2.815 Å. The approximation involved in the determination of ionic radii has two origins: 1.

The minimum in electron density between the two ions is rather ﬂat, and there is therefore some freedom of choice in determining where either of the sphere ends.

2.

The bonds in the solids considered as ionic are not always purely ionic, which can lead to slight variations from one solid to another. The ﬁrst set of ionic radii were published by Goldschmidt et al. [2] and Pauling [3], and their values are slightly diﬀerent. Table 8.2 shows the values of some ionic radii as determined by Shannon and Prewitt [4]. They showed that the values of these ionic radii depend on the coordination number (the number of nearest neighbors) of these ions. The values indicated in the table are those for coordination number 6.

The consistency of these values can be tested by comparing, as in Table 8.3, the anion–cation distances derived from these values and the distances measured in crystals with the NaCl structure, where these ions have coordination 6. In Table 8.2, the ions on a given row have the same electronic conﬁguration (the same number Z of electrons) as the rare gas shown on the same row. The charge of the nucleus increases from left to right, and consequently the attraction by the nucleus increases, which explains that the ionic radius decreases. In a given column, the ions have the same charge and, from top to bottom,

Chapter 8 – Chemical bonds and crystal structures

167

the charge of the nucleus increases, which tends to bring the electrons closer to the center, but the increase in the number of electrons tends to increase the volume of the ion. Table 8.2: Values, in Å, of some ionic radii in crystals, after [4] Ionic charge

2–

1–

Rare gas

1+

2+

He (Z = 2)

Li 0.74

Be 0.35

3+

O 1.40

F 1.33

Ne (Z = 10)

Na 1.02

Mg 0.72

Al 0.53

S 1.84

Cl 1.81

A (Z = 18)

K 1.38

Ca 1.00

Sc 0.73

Se 1.98

Br 1.96

Kr (Z = 36)

Rb 1.49

Sr 1.16

Y 0.90

Te 2.21

I 2.20

Xe (Z = 54)

Cs 1.70

Ba 1.36

La 1.06

Table 8.3: Comparison of the values of the anion–cation distances calculated from Table 8.2 and measured by X-ray diﬀraction (these values are from [5]) Compound

Calculated Measured distance distance

LiF

2.07

2.01

LiCl

2.55

2.565

LiBr

2.70

2.75

LiI

2.94

3.00

NaF

2.35

2.31

NaCl

2.83

2.815

NaBr

2.98

2.985

NaI

3.22

3.215

KF

2.71

2.67

KCl

3.19

3.145

KBr

3.34

3.30

KI

3.58

3.53

168

Symmetry and Physical Properties of Crystals

The competition between these two eﬀects explains why the ionic radius increases relatively little with atomic number Z. From Li+ to Cs+ the number of electrons grows from 2 to 54, a 27-fold increase (i.e. 33 ) while the ionic radius is multiplied, not by 3, but only by 2.3. Note: the forces involved are central, and thus independent of the bond direction, so that the various bonds of a given atom have no preferred relative orientation. The consequence is that the number of bonds between an atom and its ﬁrst neighbors can have any value, but is restricted by steric eﬀects. The structure of ionic crystals is thus characterized by the alternation of positive and negative ions, maximum compacity consistent with the respective ionic radii.

8.2.2. Bonding energy Consider again the NaCl crystal, known to have a face-centered structure (Fig. 8.3b). The Coulomb interaction energy between two ions Na+ and Cl− located a distance r from each other is given by ECoul = −e2 /r where e2 = q 2 /4πε0 , q being the electron charge and ε0 the electrical permittivity of vacuum. The bonding energy of a Na+ ion in a NaCl crystal can be calculated using the actual environment of the ion. We see on Figure 8.3 that a Na+ ion + distance r0 (ﬁrst neighbors), by 12 is surrounded by 6 Cl− ions at a √ √ Na ions − (second neighbors) at distance r0 2, by 8 Cl ions at distance r0 3, etc. The total Coulomb energy of a Na+ ion is therefore:

8 e2 e2 12 ECoul = − 6 − √ + √ − . . . = −α r0 r0 2 3 where α is called the Madelung constant of NaCl. The series which must be summed to obtain α is an alternating, slowly converging series. Computing it accurately requires special approaches. For NaCl (and for any other face-centered cubic structure of the AX type, where the ions A and X are monovalent) the value of α is 1.748, so that ECoul = −1.748

e2 . r0

For other structures, other values of α are obtained. We note that the same result would be obtained by considering a Cl− ion and its neighbors. The value of r0 is obtained from the lattice parameter a determined by X-rays, viz. a = 5.63 Å for the cubic cell of NaCl and r0 = a/2 = 2.815 Å. The value deduced for ECoul is −8.92 eV, hence an attractive energy of 8.92 eV per ion. If we take into account the repulsive energy, we obtain 7.89 eV. The binding energy measured from the heat of sublimation is 7.86 eV, in very good agreement considering the simplicity of the model.

Chapter 8 – Chemical bonds and crystal structures

Cs+

Cl–

(a)

Na+

Cl–

(b)

169

Zn2+

S2–

(c)

Figure 8.3: Examples of structures of ionic crystals with formula AX: (a) cesium chloride CsCl, primitive cubic; (b) sodium chloride NaCl (rocksalt), fcc; (c) zinc sulﬁde ZnS, fcc. In each of these structures, the motif consists of one anion–cation neighbor couple.

8.2.3. Ionic structures with formula AX The simplest and most frequent of these are the CsCl, NaCl and ZnS-type structures, shown on Figure 8.3. The CsCl structure is primitive cubic (Fig. 8.3a). The motif consists of a Cs+ ion and a Cl− ion. The Cl− ions are at the cube apices and the Cs+ ions at the cube centers. It can just as well be described by assuming the Cs+ ions are at the apices and the Cl− ions at the centers of the cubes. The NaCl (rocksalt) structure is face-centered cubic, the motif consisting of one Na+ and one Cl− ion (Fig. 8.3b). The Cl− ions are at the apices of the cube and at the face centers, and the Na+ ions at the middle of the sides and one at the center of the cube. The structure can also be described by replacing the Cl− ions by the Na+ ions and vice versa. In the zinc blende (or sphalerite) structure,1 ZnS is face-centered cubic (motif consisting of one Zn2+ ion and one S2− ion), with the S2− ions at the vertices of the cubes and at the face centers (Fig. 8.3c). If the cube is thought to be divided into eight small cubes with half the side, we see that the Zn2+ ions are at the centers of every other of these cubes. As above, the structure can also be described by substituting the S2− ions for the Zn2+ ions and vice versa. We will attempt to “predict” these simple structures with AX formula using the maximum compacity criterion. We saw that the motif is one AX unit. We will therefore consider that the ions of one type (say the negative A ions, and we will see this is reasonable), with radius r− , form a compact lattice of ions (simple cubic ﬁrst, then face-centered cubic), and determine the size of the voids in these structures where the X ions, with radius r+ , could be located. We call a the parameter of the cubic unit cell.

1. It is necessary to specify “blende structure” because ZnS can also crystallize in another form, wurtzite (Exercise 8.3).

170

Symmetry and Physical Properties of Crystals

Primitive cubic lattice The ions located at the cube apices touch each other and their radius r− is equal to a/2. The ion lattice thus formed exhibits voids centered at the centers of the cubes. The radius r+ of the sphere which can be placed at the√center of a cube while touching the ions with radius r− is such that 2r+ = a 3 − a. Hence the ratio of ionic radii should be: r+ √ = 3 − 1 = 0.73. r− The positive ion, at the center of the cube, has eight neighbors at the same distance: it has coordination number 8, and the same applies for the negative ions. Face-centered cubic lattice

√ The ions touch each other along the face diagonals, and r− = a 2/4. There are two kinds of voids: 1.

At the center of the cube: This is called an octahedral site because the ﬁgure formed by the six nearest neighbors located at the face centers is an octahedron, the regular polyhedron with eight faces. We would easily see, by considering the whole lattice, that the same type of site exists at the middle of the sides. Such a face-centered cubic lattice, where2 one type of ions is at the lattice nodes and the other type of ions at the center of the cube and at the middle of the sides, describes the NaCl structure (Fig. 8.3b). The Na+ and Cl− ions have coordination number 6.

2.

At the centers of the eight cubes with side a/2 into which the cube with side a can be divided. These are called tetrahedral sites because the ﬁgure formed by the nearest neighbors is a regular tetrahedron. In such a structure, there are twice as many tetrahedral voids as there are atoms at the apices of the cube and at the face centers, and the AX structure uses only every other void. This is the ZnS structure.

A simple geometrical calculation provides the radius ratios for the two kinds of voids: r+ = 0.41 r− r+ = 0.22 r−

for the octahedral site (coordination number 6), for the tetrahedral site (coordination number 4).

Let us now see how the various voids are ﬁlled depending on the value of the r+ /r− ratio. If r+ /r− = 0.73, the negative ions are at the vertices of the cubes and the positive ions at the centers of the cubes: this is the CsCl structure (Fig. 8.3a). 2. This description implies that we chose to have a lattice node coincide with one type of ion.

Chapter 8 – Chemical bonds and crystal structures

171

The more r+ /r− exceeds the value 0.73, the more the positive ion moves the negative ions apart. If r+ /r− is smaller than 0.73, the positive ion ﬂoats about in the void, and the negative ions rearrange into a face-centered cubic lattice where the positive ion sits in the octahedral void, which it enlarges by moving the negative ions apart (NaCl structure on Fig. 8.3b). If r+ /r− = 0.41, the negative ions touch one another. The more r+ /r− exceeds the value 0.41 (while remaining < 0.73), the more the positive ion pushes the negative ions apart. When r+ /r− is less than 0.41, the positive ion ﬂoats about in the octahedral cavity and the positive ions move to the tetrahedral sites (ZnS-blende structure of Fig. 8.3c), moving apart the negative ions, which come to contact only when r+ /r− further decreases to the value 0.22. To summarize, we obtain the following rule: if r+ /r− > 0.73, CsCl structure; if 0.41 < r+ /r− < 0.73, NaCl structure; if 0.22 < r+ /r− < 0.41, ZnS (blende) structure. This rule is quite well obeyed (Table 8.4). The deviations originate mainly from the fact that the bonds are but rarely purely ionic, in contrast with the starting assumption. There can be for example a covalent contribution, which leads to a tendency for the external electrons not to be distributed with spherical symmetry, so that the starting hypothesis of a spherical ion is no more perfectly satisﬁed. Table 8.4: r + /r − ratios for some crystals with various cubic structures CsCl type

r+ /r−

NaCl type

r+ /r−

CsCl

0.94

KF

1.04

CsBr

0.87

CaO

0.71

CsI

0.77

KBr

0.70

LiF

0.56

ZnS type

r+ /r−

NaCl

0.56

AgI

0.52

CaS

0.54

ZnS

0.40

MgO

0.51

BeS

0.19

LiBr

0.38

8.2.4. Other cubic structures It appears useful to introduce a few other ionic structures, considered as “classic” because many crystals share one or the other of these structures, which are so to speak canonical structures. We chose ﬂuorite CaF2 , rutile TiO2 ,3 and the perovskite structure CaTiO3 . 3. TiO2 also exists in two other forms: anatase (tetragonal) and brookite (orthorhombic).

172

Symmetry and Physical Properties of Crystals

The CaF2 structure is face-centered cubic (Fig. 8.4a). The Ca2+ ions occupy the apices and the face centers of the cube, and the F− ions the eight tetrahedral sites. This structure can also be described as a set of cubes, with sides half the side of the unit cell, where the apices are occupied by a ﬂuorine ion and the center of every other cube by a Ca2+ ion. The ratio of the ionic radii of Ca2+ and F− is equal to 0.74, in good agreement with the coordination number 8 corresponding to a positive ion at the center of a cube whose apices are occupied by a negative ion as for CsCl. However here, since there are twice as many F− ions as Ca2+ ions, the Ca2+ ions are at the centers of every other cube only. The result is a face-centered cubic unit cell.

F

Ca

(a)

Ti

(b)

O

Ca

Ti

O

(c)

Figure 8.4: Three examples of structures representative of many ionic crystal structures: (a) ﬂuorite CaF2 ; (b) rutile TiO2 ; (c) CaTiO3 , the perovskite structure Rutile TiO2 has a tetragonal primitive unit cell (Fig. 8.4b). The Ti atoms are located at the vertices and at the center of the unit cell. Each of the apical Ti atoms is surrounded by two O atoms at the same height, and the Ti atom and its two O neighbors are aligned parallel to one of the diagonals of the square base of the unit cell. The Ti atom at the center of the unit cell also has two O atoms at the same height as itself, but they are aligned parallel to the other diagonal of the square. The perovskite structure, the model of which is CaTiO3 (Fig. 8.4c), is primitive cubic with Ca atoms at the apices of the cube, O atoms at the face centers, and a Ti atom at the center of the cube. The structure of CaTiO3 actually is slightly distorted with respect to this cubic structure. Many substances have this type of pseudo-cubic unit cell, and they often exhibit a high-temperature phase which is exactly cubic. A good example is barium titanate BaTiO3 , which is cubic at high temperature (T > 120◦ C), and undergoes, when temperature decreases, various transitions toward other structures: ﬁrst tetragonal, then orthorhombic and ﬁnally rhombohedral (Exercise 12.7).

Chapter 8 – Chemical bonds and crystal structures

173

8.3. Covalent bonds 8.3.1. Nature of covalent bonds In an elementary presentation, we can say that covalent bonding occurs between two atoms when they share a pair of electrons. In contrast to the ionic bonds, the electron density is no more zero between the atoms. The nature of this bond can only be explained through quantum mechanics. To give a taste of the argument, take the simplest example, that of the H+ 2 ion consisting of two protons and an electron. It can be shown that the wave function of the electron can be written as the combination of the atomic wave functions or “orbitals” Ψ1 and Ψ2 of each of the hydrogen atoms: Ψ± = A± (Ψ1 ± Ψ2 ). The probability density of the electron between the nuclei is non-zero for the Ψ+ combination (called the bonding solution) while that associated to the Ψ− combination (called the antibonding solution) is zero. The energies E + and E − associated to these two states vary as a function of the distance ρ between the protons as shown on Figure 8.5. The energy E + is always smaller than E − , and its minimum value −E0 leads to a cohesive energy equal to E0 . Each state of the bonding orbital can be occupied by two electrons with opposite spins (Pauli’s principle). In the ground state of the neutral hydrogen molecule (H2 ), the electrons of both atoms occupy the bonding state, and they have opposite spins. This is the prototype of the covalent bond, consisting of two electrons with opposite spins, shared between the two bound atoms. If the external electron shell of an atom is several electrons short of being full, this atom can share electrons with several neighboring atoms and thus form several covalent bonds. Each covalent bond then requires the participation of one orbital per bound atom. Energy

E+

E−

0 −E 0

Figure 8.5: Schematic representation of the potential energy of an H+ 2 ion as a function of the distance ρ between the hydrogen nuclei for the bonding orbital, E + , and the anti-bonding orbital, E −

174

Symmetry and Physical Properties of Crystals

8.3.2. Basic property It can be shown that a covalent bond is the more stable the larger the overlap between the wave functions of the two electrons that take part in the bond. The electronic states of isolated atoms do not all have the spherical symmetry of s states. The p states, with 3-fold orbital degeneracy (the total degeneracy, with spin included, is then 6-fold) have wave functions which point along the three axes of an orthogonal referential. There is thus a strong overlap of the p orbitals with the orbitals of the neighboring atoms if the latter are located along these axes. Consider the example of the nitrogen–hydrogen bond in the NH3 molecule. The electronic structure of the nitrogen atom includes two 1s electrons, two 2s electrons and three 2p electrons. The external 2p shell of the nitrogen atom lacks three electrons to be complete. The three p orbitals of the nitrogen atom each form a covalent bond with the spherical 1s orbital of one of the hydrogen atoms. These bonds are almost at right angles to one another. Actually, the angle between two bonds is 107◦ , and the molecule is a pyramid, the base of which is an equilateral triangle and the apical angles are equal to 107◦ . The N atom is at the apex of the pyramid and the H atoms at the apices of the equilateral base. In general, the principle of maximum overlap of wave functions leads to the covalent bonds having preferential directions.

8.3.3. Examples The following examples are monoatomic crystals. The bonds therefore connect atoms of the same type. Diamond It consists of carbon atoms. The electronic structure of the outermost shell of carbon (n = 2) consists of two 2s electrons and two 2p electrons. It lacks four electrons to be full. The four electrons of the n = 2 shell form hybrid orbitals consisting of linear combinations of the s, px , py and pz orbitals. These orbitals, called sp3 , are oriented along the directions that connect the center of a regular tetrahedron to its four apices. In a diamond crystal, each carbon atom is thus connected to four neighbors by tetrahedral bonds (Fig. 8.6). The diamond crystal can be considered as a giant molecule, with practically inﬁnite extent. Silicon and germanium crystals have the same structure as diamond. Their outermost shell (n = 3 for Si and n = 4 for Ge) also includes 4 electrons (two s electrons and two p electrons). Generally, consider atoms in which the outermost shell would have 8 electrons if it were saturated. If this shell actually contains N electrons, the external shell will be saturated if 8 − N covalent bonds are formed. Each bond then uses one of the N electrons of the neighboring atom (an atom of the same type

Chapter 8 – Chemical bonds and crystal structures

175

in the monoatomic crystals to which we restrict discussion), and this requires N ≥ 8 − N , hence N ≥ 4. The following paragraphs successively discuss a case where N = 5, then a case with N = 6. An example with N = 7 is treated in Section 8.4.2.

Figure 8.6: Crystal structure of diamond Arsenic The outermost electronic shell (n = 4) contains two 4s electrons and three 4p electrons, hence a total of ﬁve electrons. Three pseudo-plane bonds are then formed, and the pseudo-planes can be described as corrugated planes. An atom located in the zero height plane is connected to three atoms at height 1.37 Å as shown on Figure 8.7, which represents the projection of these atoms onto the plane at height zero. The arrows indicate the direction of increasing height on the bonds. The angle between bonds is 94.1◦ (instead of 120◦ as expected for coplanar bonds). The next corrugated plane is at height 3.516 Å and its projection is displaced with respect to the ﬁgure by vector AB. The “corrugated” planes are bound to one another by Van der Waals bonds (see next section).

A

B

3.76 A°

Figure 8.7: Arsenic crystal; structure of a pseudo-plane of atoms. The atoms represented by empty circles are at height zero and those represented by full circles at height 1.37 Å. Selenium The outermost electronic shell (n = 4) contains six electrons (two 4s electrons and four 4p electrons), and each Se atom must therefore share two bonds. They are at an angle of 103.1◦ to each other. The “inﬁnite molecule” is a chain (Fig. 8.8). The positions of the atoms in one chain are deduced from

176

Symmetry and Physical Properties of Crystals

one another by the symmetry elements of a 31 screw axis. These helix-shaped chains are stacked parallel to one another and they are bound to one another by Van der Waals forces. 1⁄3

1⁄3 0

0

2⁄3

C

2⁄3

b 1⁄3

1⁄3 0

a

2⁄3

(a)

0 2⁄3

(b)

Figure 8.8: Selenium crystal: (a) structure of a chain of atoms and its 31 screw axis; (b) hexagonal unit cell projected on its basal plane, with the height of the atoms expressed in units of the lattice parameter c

8.3.4. Conclusion 1.

Covalent bonds are oriented: this is their main characteristic.

2.

The distance between two given atoms engaged in a covalent bond is well deﬁned. For example, the C–C distance in a diamond crystal is equal to that between carbons in the single bond of ethane (C2 H6 ), 1.54 Å.

3.

The order of magnitude of the energy of these bonds is a few eV. Examples are given in Table 8.5. Table 8.5: Energy of some covalent bonds. The C–C bond considered is a single bond.

Energy (in eV) 4.

H–H

C–C

Si–Si

Ge–Ge

4.5

3.6

2.3

1.9

There are many solids where the bonds are not totally covalent but partly ionic: they are referred to as iono-covalent bonds. The atoms engaged in these bonds always ﬁll their outermost electronic shell.

Chapter 8 – Chemical bonds and crystal structures

177

8.4. Van der Waals bonds, or molecular bonds 8.4.1. Nature and properties The simplest example is that of the rare gases, consisting of neutral atoms with their outermost electronic shell full. Although the atoms are neutral, the Van der Waals force is electrostatic in origin. These atoms do not have a permanent electric dipole moment (P(t) = 0) but the dipole moment oscillates around its average zero value. At a given time P(t) is therefore non-zero, and it creates an electric ﬁeld at the position of the neighboring atom, which it polarizes. The interaction energy between the two atoms can be calculated. It is found to be negative, with absolute value proportional to 1/r 6 , whence an attractive force varying as 1/r 7 . The order of magnitude of the Van der Waals type bond energies is 0.1 eV. There is no restriction on the angles between bonds, which may have any orientation. Van der Waals radii: They can be determined from the contacts between identical atoms bound by Van der Waals forces. Then, knowing a number of these radii, we can determine the others by examining the distances between atoms of diﬀerent types bound by a Van der Waals force.

8.4.2. Example Van der Waals bonds appear in all crystals where the elementary building block is a molecule. A very simple example is the chlorine crystal (Fig. 8.9). 0

½

0

c

0

½

0

½

0

½

b 0

½

0

½

0

½

0

½

0

Figure 8.9: Orthorhombic crystal of chlorine: projection of the atoms onto a plane perpendicular to basis vector a. The lines connecting two chlorine atoms represent the covalent bonds.

178

Symmetry and Physical Properties of Crystals

The outermost shell of the chlorine atom has 7 electrons, and the atom can covalently bond only to one neighbor to form a Cl2 molecule. The crystal consists of Cl2 molecules connected by Van der Waals forces. This is called a “molecular crystal”. The molecule is extremely simple in this case, but in general the molecules can contain a great number of atoms and have complicated, irregular shapes. Their most compact stacking is not easily determined, all the more since other factors can play a part, for example local charges which create a local electric ﬁeld in their vicinity.

8.5. Metallic bonds 8.5.1. Nature and properties In a pure metal, the atoms are all identical and the bond cannot be ionic. Also, the number of electrons in the outermost shell of a metal atom is smaller than 4, and the bond cannot be covalent. The nature of the metallic bond can be understood starting from the crystal structure (as evidenced by X-ray diﬀraction), and describing quantum mechanically the behavior of an electron in the periodic potential of the metal ions that form the crystal lattice. It can then be shown, for the electrons in a crystal, that there is a set of energy levels forming a continuous band called the conduction band. The electrons in the conduction band behave almost like free electrons, and they also provide the bonding between all the atoms. The crystal structures observed are well explained by a model of hard spheres with compact (close-packed) stacking. The radius of the spheres is calculated as half the distance between neighboring atoms, as deduced from the crystal structure determined by X-ray diﬀraction. The radius of the metallic ions thus determined is always larger than the radius of the corresponding ion in an ionic crystal. For example the radius of the Na+ ion is equal to 1 Å while the radius of Na metal is 1.86 Å. The interpretation is that, in NaCl for example, the Na+ ions are attracted by the Cl− ions and therefore get as close as they can to them. In metallic Na, the Na+ ions are repelled, cohesion being due to the conduction electrons. The cohesive energy of a metal is of the order of 1 eV per atom (except for the transition metals).

8.5.2. Examples The maximal compacity of a stacking of identical hard spheres is obtained for the face-centered cubic and close-packed hexagonal structures.

Chapter 8 – Chemical bonds and crystal structures

179

Consider two spheres with radius a, touching each other. A third sphere contacting these two spheres will form with the two ﬁrst ones an equilateral triangle. A plane of contacting spheres, where the centers are designated as A, form a lattice of plane hexagonal unit cells (Fig. 8.10a), and the lines connecting the centers of the spheres form a set of equilateral triangles. A sphere will position above this plane in the most compact way possible if its center projects at the center of any one of these equilateral triangles. Since there are twice as many centers of equilateral triangles as there are spheres in the compact starting plane, the contacting spheres in the second plane will project on every other of these two sites, which we call B. We will call C sites those which project on the other centers of equilateral triangles. The spheres of the third compact plane can now project either on the C sites or on the A sites. In the ﬁrst case the crystal will consist of the succession of planes ABCABCABC. . . , while in the second case the succession will be ABABABAB. . . It is easy to show (Exercise 8.1) that the atoms corresponding to succession ABCABC. . . form a face-centered cubic lattice (the motif consisting of a single atom). The planes A, B and C are parallel to the (111) planes of this structure. In the case of the ABABAB. . . sequence, the atoms form a hexagonal lattice. The a and b vectors of the hexagonal lattice are the basis vectors of the plane hexagonal starting lattice. Vector c, perpendicular to a and b, has for its length the distance between two successive A (or B) planes. A simple geometrical calculation (Exercise 8.2) shows that the c/a ratio is then 2 2/3 = 1.63.

b

b a

(a)

A B C

a

(b)

Figure 8.10: Compact stacking of spheres: (a) plane of contacting spheres; (b) projection onto this plane of the atom positions in the neighboring planes Table 8.6 shows that most metal structures are indeed either face-centered cubic or hexagonal, but in the latter case with more or less compacity. However there are also body-centered cubic (I) structures. Some metals are polymorphic, i.e. they feature various structures depending on temperature: this is the case for iron, where γ Fe has an F lattice and α Fe an I lattice. It turns out, when calculated, that the ionic radii are in this case close to each other.

180

Symmetry and Physical Properties of Crystals Table 8.6: Structure and lattice parameters of some metals Face-centered cubic lattice

Body-centered cubic lattice

Hexagonal lattice

Element

a (Å)

Element

a (Å)

Element a (Å)

c (Å)

c/a

Ag

4.086

Cr

2.884

Be

2.287

3.583

1.566

Al

4.050

Fe α

2.8665

Co α

2.507

4.069

1.623

Au

4.078

Li

3.509

Cr

2.722

4.427

1.626

Co

3.548

Mo

3.147

Mg

3.209

5.210

1.624

Cu

3.615

Na

4.291

Ni

2.65

4.33

1.634

Feγ

3.591

Nb

3.300

Ti

2.95

4.686

1.588

Ni

3.524

Zr

3.62

Zn

2.665

4.947

1.856

8.6. Remarks and conclusions We described the various types of bonds between atoms in a crystal. However, bonds are not always of a perfectly well-deﬁned type. In particular, covalent and ionic bonds are only the extreme terms of a set of bonds featuring both an ionic and a covalent character. Also, several types of bonds can appear together in a crystal: we saw examples of coexistence of covalent binding and Van der Waals binding in crystals of arsenic, selenium and chlorine. To conclude, we give two examples of simple crystals exhibiting strong anisotropy because they consist of plane layers bound to one another by weak Van der Waals bonds while the binding within the layers have mixed character and higher energy by at least an order of magnitude. Graphite crystal It consists of carbon atoms each of which is connected to three other carbon atoms by covalent bonds (sp2 hybridization between the s, px and py orbitals), within planes with hexagonal structure (Fig. 8.11). The fourth valence electrons, with orbital pz , of two neighboring atoms bind to each other through a mainly covalent bond. This bond is partly metallic and is delocalized along the plane. This partly metallic character explains the non-negligible electrical conductivity measured along these planes (see Sect. 9.3.1). The inter-plane binding is Van der Waals type.

Chapter 8 – Chemical bonds and crystal structures

181

3.35 Å

1.42 Å

Figure 8.11: Structure of graphite GeS2 crystal The layers consist of a set of tetrahedra. The center of each tetrahedron is occupied by a germanium atom, and the apices by sulfur atoms. Within a layer, the Ge atoms form a plane, and the tetrahedra are connected to one another through their apices. Each sulfur atom at the apex of a tetrahedron is thus connected to two Ge atoms. The Ge–S bonds are iono-covalent, and the layers are bound to one another by Van der Waals forces.

8.7. Exercises Exercise 8.1 Lattice for an ABCABC close-packed stacking. Comparison of Figures 8.10b and 3.14c shows that the spheres in an ABCABC stacking form a rhombohedral lattice. Show that this rhombohedral lattice is a face-centered cubic lattice. Exercise 8.2 Lattice for an ABABAB close-packed stacking 1.

In this stacking the centers of a sphere in plane B and of its three contacting spheres in plane A form a regular tetrahedron with side a equal to the length of the basis vector a of the hexagonal unit cell. Determine, as a function of a, the distance h between planes A and B.

2.

Calculate the c/a ratio for the hexagonal unit cell of the ABABAB lattice.

Exercise 8.3 Tetrahedral sites In the close-packed stacking modes ABCABC and ABABAB, one atom in a given layer and its three nearest neighbors in the adjacent layer form a regular tetrahedron.

182

Symmetry and Physical Properties of Crystals

1.

Calculate the distance d between the center of this tetrahedron and each of its apices.

2.

A spherical atom (or ion), with radius r1 , is placed at the center of this tetrahedron so that it contacts the atoms of the close-packed stacking with radius r2 . Calculate the ratio r1 /r2 .

3.

Wurtzite is a crystal form of ZnS diﬀerent from blende. Its lattice is hexagonal, with a = 3.811 Å, c = 6.234 Å. The atom positions in the unit cell are: Zn

0, 0, 0

S

0, 0, u

1 3, 1 3,

2 3, 2 3,

1 2 1 2

+u

and

u ≈ 0.375.

Show that the sulfur atoms are practically in the tetrahedral sites of a structure in which the centers of the Zn atoms form an ABABAB stacking. Compare this to the blende structure described in Section 8.2.3.

Chapter 8 – Chemical bonds and crystal structures

183

Complement 8C. Magnetic structures Understanding the physics of magnetic materials requires a knowledge not only of their crystal structure but also of their magnetic structure. The crystal structure indicates the shape and dimensions of the unit cell, the positions of the various individual ions or atoms, and the extent of their thermal vibration. The magnetic structure describes the size and orientation of the magnetic moment carried by some of the ions. Materials are often designated as magnetic when they react strongly to an applied ﬁeld. This usually means that they contain permanent magnetic moments which are, below a transition temperature, ordered. The simplest magnetic materials are ferromagnets: below TC , the Curie temperature, all the magnetic moments are, within a magnetic domain,4 parallel (Fig. 8C.1a).

(a)

(b)

(c)

(d)

Figure 8C.1: Schematic representation of the magnetic moment arrangements, on a microscopic scale, in ferromagnets (a), ferrimagnets (b) and antiferromagnets (c). In these ﬁgures, each arrow represents an atomic magnetic moment. Figure (d) shows, on a macroscopic scale, an arrangement of magnetic domains in a ferromagnet: each arrow then represents the direction of the spontaneous magnetization:5 the scale of this ﬁgure could be anywhere between micrometers and millimeters.

4. A magnetic domain is a macroscopic region of the sample where the orientation of the spontaneous magnetization, hence of the magnetic moments, is uniform. There are always at least two opposite (time-reversed) directions for the magnetic moments, as in uniaxial materials. The number of equivalent domains is set by the ratio of the magnetic point symmetry of the material above and below the Curie temperature, and it depends on what crystallographic direction the moments spontaneously take. For example, when the material is cubic above the Curie temperature and the spontaneous magnetization directions are <100>, as in slightly silicon-alloyed iron, there are 6 families of magnetic domains (spontaneous magnetization along ±[100], ±[010], ±[001]) (Fig. 8C.1d). The magnetization process, under the inﬂuence of an applied magnetic ﬁeld, starts with the growth of the favorably oriented domains. 5. The magnetization is the magnetic moment per unit volume. It is analogous to the polarization in dielectrics, discussed in Chapters 9 and 15.

184

Symmetry and Physical Properties of Crystals

Examples of ferromagnets are iron, cobalt, nickel and many of their alloys or compounds. Another important class of magnetic material comprises the ferrimagnets (Fig. 8C.1b), in which the magnetic moments of one type of ions are “up”, and those of another type of ions, with a diﬀerent value of the moment, are “down”, yielding a resulting non-zero (spontaneous) magnetization at the scale of a domain. Examples are the ferrites used in high-frequency transformer cores, or as permanent magnets. The order feature is shared by some materials which do not react strongly to a magnetic ﬁeld and are therefore not obviously attractive for applications. These have, below the ordering temperature (the Néel temperature TN ), as many “up” as “down” magnetic moments with the same modulus, and therefore zero overall spontaneous magnetization. These materials, the simpler examples of which are NiO, CoO and MnO, or MnF2 , CoF2 and NiF2 , are called antiferromagnets (Fig. 8C.1c). The prime tool for investigating the magnetic structure of materials is neutron diﬀraction. Neutrons (see Complement 4C) interact with the nuclei (the nuclear interaction) and, since they carry a magnetic moment, they also sense magnetic ﬁelds. In the wavelength range used for diﬀraction by the microscopic structure of materials, on the order of 10−10 m, they are diﬀracted by the microscopic-scale variation of the magnetic ﬁelds in matter, and the probability of magnetic scattering happens to be of the same order of magnitude as for nuclear scattering. From this information, the distribution of magnetic moments that gives rise to these ﬁelds can be determined. For example, in some simple antiferromagnets (CoO, NiO or MnO), the magnetic period, in the direction along which the moments alternate, is double that of the chemical structure, because chemically identical ions have alternately up and down orientations. The neutron diﬀraction pattern will therefore feature new, purely “magnetic” reciprocal lattice nodes and diﬀraction peaks, which vanish above the Néel temperature. Just as the symmetry of the crystal structure is described by one of the 230 space groups, the magnetic symmetry is described by one of the 1651 magnetic groups. The 32 crystallographic point groups are replaced by 122 magnetic point groups. The central addition to the toolbox of structure symmetry elements is the operation called “time reversal”. The notion under this provocative term is actually simple. Microscopic magnetic moments are represented by axial vectors (see Sect. 10.6). They are due to the equivalent of current loops, i.e. of circulating electric charge. Reversing the magnetic moment is tantamount to reversing the velocity of the charges, as if a movie were being played backwards, or if time were ﬂowing backwards. Thus the magnetic symmetry involves operations such as m (mirror combined with reversal of the magnetic moment, which can be described as time reversal), and the magnetic Bravais lattice description can feature notations such as Ip , meaning anti-centering, i.e. the combination of displacement by half the unit cell diagonal and magnetic moment reversal.

Chapter 8 – Chemical bonds and crystal structures

185

Actually, X-rays also interact, albeit weakly, with the magnetic moments. With synchrotron radiation X-rays, valuable complementary information can be extracted on magnetic structures: magnetic X-ray scattering can reveal the two contributions (spin and orbital) to the magnetic moment, whereas magnetic neutron diﬀraction is sensitive only, via the magnetic ﬁeld it creates, to the total magnetic moment.

Further reading D.H. Ryan, Neutron Powder Diﬀraction Studies of Magnetic Materials. Powerpoint document, prepared for the 2009 summer course of the Canadian Institute for Nuclear Scattering; available on the web at www.cins.ca/docs/SS09 (click on DHR CNBC June09.ppt) M. de Graef, Teaching crystallographic and magnetic point group symmetry using three-dimensional rendered visualizations, International Union of Crystallography, Teaching Pamphlets; http://www.iucr.org/ data/assets/pdf ﬁle/0006/13929/ﬁnal 23.pdf J. Rodríguez-Carvajal and F. Bourée, Symmetry and magnetic structures, in Contribution of Symmetries in Condensed Matter, ed. by B. Grenier, V. Simonet and H. Schober. Proceedings of spring school held at Presqu’île de Giens, France, in May 2009. EDP Web of Conferences, vol. 22 (2012). Available on the web, at http://dx.doi.org/10.1051/epjconf/20122200010

186

Symmetry and Physical Properties of Crystals

References [1] G. Schoknecht, Z. Naturforsch. 12A, 983 (1957) [2] V.M. Goldschmidt, T. Barth, G. Lunde, W.H. Zachariasen, Skr. Norske Vidensk. Akad. Skrifter I Mat. Naturv. Kl. 2, 1 (1926) [3] L. Pauling, J. Am. Chem. Soc. 49, 765 (1927) [4] R.D. Shannon, C.T. Prewitt, Acta Cryst. B25, 925 (1969) [5] W.G. Wyckoﬀ, Crystal Structures, vol. 1 (Wiley, 1963)

Chapter 9

Crystal anisotropy and tensors This chapter shows why the anisotropy of crystals requires a representation of their physical properties by tensors, and deﬁnes them. It then shows how the symmetry of a given crystal (its point group) inﬂuences the form of these material tensors. Curie’s and Neumann’s principles and their application to the tensor properties of crystals are presented in Section 9.5.

9.1. Introduction The physical properties of crystals belong to either of two broad categories: intrinsic and extrinsic properties. The intrinsic physical properties are identical in various samples of a given material because they depend on the very nature of the material: its chemical composition, the nature of the bonds between atoms and their structural arrangement. Examples of intrinsic properties are: thermal expansion and elastic properties, which reveal on a macroscopic scale the forces between neighboring atoms, the type of electrical conductivity (insulating or conducting or semiconductor), which is related to the nature of the chemical bonds between atoms. A good example is carbon, an insulator when it crystallizes in the form of diamond, while its other (polymorphic) form, graphite, is a conductor. The extrinsic properties are related to the existence of defects in the crystal, and they can therefore vary extensively between samples. Two examples are: plastic deformation: here, in contrast to elastic deformation, the sample does not return to its initial state when the force which created the strain is removed. Plastic deformation is related to the existence and multiplication of linear defects, called dislocation lines (or, for short: dislocations), whose initial number and nature vary from sample to sample depending on the growth process and on the previous deformation. A brief introduction to dislocations is given in Complement 13C.

© Springer Science+Business Media Dordrecht 2014 C. Malgrange et al., Symmetry and Physical Properties of Crystals, DOI 10.1007/978-94-017-8993-6_9

187

188

Symmetry and Physical Properties of Crystals the value of the electrical conductivity of a semiconductor, which depends on the density of impurities (which means, when it is deliberate, the extent of doping) in the sample.

In this book, we only consider intrinsic physical properties of crystals. In the ﬁrst part, we saw that crystals are formed from the periodic repetition of the crystal motif, at the microscopic scale, along three non-coplanar directions. A direct consequence of this periodicity is the anisotropy of the physical properties of crystals, which depend on the direction in which a constraint is applied and on the direction in which the resulting eﬀect is measured. The description of this anisotropy involves special mathematical objects, called tensors. This is why this second part of the book starts with two general chapters which analyze the notion of tensor, describe the general properties of tensors, and show how the symmetry of an individual crystal makes it possible to reduce the number of independent coeﬃcients of any tensor representing one of its intrinsic physical properties. The following chapters describe speciﬁc physical properties, mainly mechanical and optical.

9.2. Anisotropic continuous medium The physical properties discussed in this second part of the book are macroscopic properties. In describing them, the crystal is considered as a continuous and anisotropic medium. To satisfy the assumption of continuity, we must assume that any elementary volume V fulﬁlls two conditions. It must contain enough unit cells that it may be considered as homogeneous, but it also must be small enough that the variations of an external applied ﬁeld within this volume be negligible. When these external ﬁelds are sine waves (electric ﬁeld E or magnetic ﬁeld B. . . ), the characteristic length is their wavelength λ. The elementary volume V must therefore have dimensions very much smaller than this wavelength. The two above conditions can be summarized by the double inequality: √ 3 a V λ where a is the largest one among the parameters of the crystal unit cell. This means that, if the wavelength of the applied ﬁelds is much larger than the dimensions of the unit cell, the variations of the ﬁeld within the elementary volume can be neglected, and the crystal can be viewed as a continuous medium. Furthermore, the cell parameters can be considered as inﬁnitely small with respect to the relevant volume, and the same applies even more to fractions of these parameters. It is therefore no more justiﬁed to distinguish between pure and screw rotation axes, or between pure and glide mirrors, since the translations associated to these symmetry elements are fractions of a lattice parameter (see Sect. 7.2.1 and 7.2.2). In other words, the eﬀect of the crystal’s symmetry on its macroscopic properties will be described by its point group and not by its space group.

Chapter 9 – Crystal anisotropy and tensors

189

Conversely, if the wavelength of the ﬁeld applied to the crystal is on the same order of magnitude as its lattice parameter (X-ray range), the crystal can no more be considered as continuous. Its discrete structure must be taken into account, and indeed such probes can be used to investigate the crystal structure and thus the space group of the crystal. Our discussion of the physical properties will involve either static constraints (mechanical properties), or periodic constraints with wavelengths larger by several orders of magnitude than the lattice parameters (acoustic waves and optical electromagnetic waves). The crystal can thus be considered as an anisotropic continuous medium, and crystal symmetry aﬀects the physical properties through the point group of the crystal.

9.3. Representing a physical quantity by a tensor Some physical quantities are independent of any notion of orientation: this is the case for temperature or the mass per unit volume of a material. They are expressed by a scalar. Others are expressed by a vector, for example an electric ﬁeld or the polarization of a crystal under the inﬂuence of this ﬁeld. Consider two vector-type physical quantities, A and B, related by a linear law. In a gas or liquid, this relation is written as A = γB where γ is a scalar. A and B are then parallel. In a crystal, A is generally not parallel to B, and a tensor must be introduced to describe the physical quantity γ. This will be analyzed in detail on the basis of an example in the next section (Sect. 9.3.1). Tensors, in the same way as vectors which, as we will see, are just a special form of tensors, are deﬁned by their components in a given system of axes. It is simpler, and this will be done throughout this book, to select for this use not the set of crystal axes (basis {a, b, c}), but an orthonormal set of axes (Ox1 x2 x3 ) (basis {e1 , e2 , e3 }), usually chosen as close as possible to the crystal axes. For example, in the case of the crystal systems with an orthogonal unit cell (orthorhombic, tetragonal, cubic), the orthonormal set of axes (Ox1 x2 x3 ) in which we express the tensor is chosen parallel to the vectors a, b, c that deﬁne the unit cell. For crystals with a hexagonal unit cell, one of the axes is chosen parallel to the 6-fold axis of the lattice, etc.

9.3.1. Example: electrical conductivity Electrical conductivity is a good example for understanding the eﬀect of crystal anisotropy on the physical properties of a crystal. An electric ﬁeld E applied to a conductor induces a current density j within the material. The motion of free charges is then characterized by the electrical conductivity σ through j = σE where σ is a scalar if the material is isotropic.

(9.1)

190

Symmetry and Physical Properties of Crystals

To illustrate this relation, imagine we are performing conductivity measurements on two very diﬀerent samples of graphite: a compacted graphite powder, and a single crystal of graphite. The crystal structure of graphite, as described in Chapter 8 (Fig. 8.11), consists of a stacking of equidistant dense planes, with hexagonal symmetry, called graphitic planes, connected by Van der Waals bonds. In the ﬁrst experiment, performed on compacted powder, we apply an electric ﬁeld E in any direction. The current density turns out to be parallel to E whatever the direction of the applied ﬁeld E, and proportional to the norm of E. The conductivity σ is then a scalar. In this case, the powder behaves with respect to the applied electric ﬁeld like an isotropic material. The powder consists of many small crystals, randomly oriented relative to one another, and thus the inﬂuence of structural anisotropy on the measured physical property disappears. Now consider the single crystal of graphite. Due to the special structure of this material, very diﬀerent values of the current density will be obtained depending on the orientation of the applied electric ﬁeld. A strong current density will be measured if the ﬁeld is applied along a direction in the graphitic planes, and a weak current density will be obtained with the ﬁeld perpendicular to the graphitic planes (Sect. 8.6). The ratio between these values varies between 102 and 105 depending on crystal quality [1]. If the applied ﬁeld has a general direction, the current density has no reason to be parallel to the ﬁeld, and the three components of j can be expressed as a function of those of E through the linear relations: j1 = σ11 E1 + σ12 E2 + σ13 E3 j2 = σ21 E1 + σ22 E2 + σ23 E3

(9.2)

j3 = σ31 E1 + σ32 E2 + σ33 E3 , where ji and Ei with i = 1, 2, 3 are the components of j and E respectively, in an orthonormal set of axes (Ox1 x2 x3 ). These three relations can also be written ji =

3

σik Ek

k=1

or, using Einstein’s condensed notation, also referred to as Einstein’s convention: ji = σik Ek . This convention consists in suppressing the sum sign, which becomes implicit, before a product of factors when the sum is performed over a subscript that appears twice in the product. Here the summation is performed over subscript k (called the dummy subscript, or dummy index), which appears in σik and in Ek . The subscript i, which is not summed over, is called the free subscript, and it must appear on both sides of the equal sign. We will always use this notation in what follows.

Chapter 9 – Crystal anisotropy and tensors

191

Equations (9.2) can also be written in the following matrix form: ⎞ ⎛ ⎞⎛ ⎞ ⎛ σ11 σ12 σ 13 E1 j1 ⎝ j2 ⎠ = ⎝ σ21 σ22 σ23 ⎠ ⎝ E2 ⎠ . j3 σ31 σ32 σ33 E3 Electrical conductivity clearly appears as a table of 3 × 3 = 9 components of a quantity described as a tensor quantity. The nine numbers that deﬁne it depend on the axis system chosen to express the components of vectors E and j. It is therefore essential to understand how this table transforms when the vectors E and j are expressed in another orthonormal coordinate system. In other words, we must determine the relation that makes it possible to go over from table σik , obtained when the vectors E and j are expressed in a obtained when the same vectors are given orthonormal frame, to the table σik expressed in another orthonormal frame.

9.3.2. A refresher on orthonormal frame changes Let R be a frame deﬁned by the orthonormal basis {e1 , e2 , e3 } and R a new frame deﬁned by the orthonormal basis {e1 , e2 , e3 }. The new basis vectors can be expressed as a function of the old ones through the relations: ei = aij ej

(9.3)

where we use Einstein’s convention as deﬁned in the section above: summation over the subscript j which appears twice is implicit. We immediately see that: aij = ei · ej .

(9.4)

Equation (9.3) can be represented through the table below: e1

e2

e3

e1

a11

a12

a13

e2

a21

a22

a23

e3

a31

a32

a33

In this table akl = ek · el . We note that aji = ej · ei is the projection of ei onto ej , so that: ei = aji ej .

(9.5)

192

Symmetry and Physical Properties of Crystals

A vector x can be expressed in basis {e1 , e2 , e3 } through relation: x = x1 e1 + x2 e2 + x3 e3

or

x = xi ei

(9.6)

or

x = xj ej .

(9.7)

and in basis {e1 , e2 , e3 } through x = x1 e1 + x2 e2 + x3 e3

Taking relation (9.5) into (9.6), we obtain x = xi aji ej and, comparing with (9.7), we obtain xj = aji xi .

(9.8)

In the same way, taking (9.3) into (9.7) and comparing with (9.6), we obtain xj = aij xi .

(9.9)

Transformation from one orthonormal frame to another orthonormal frame leads to the two following relations, (9.10) and (9.11): aih aik = δhk

(9.10)

where δhk is Kronecker’s symbol, equal to 1 if h = k and to 0 if h = k. The proof is that eh · ek = δhk = aih ei ajk ej = aih ajk δij = aih aik . In the same way, using the fact that eh · ek = δhk , we obtain ahi aki = δhk .

(9.11)

Let us designate as A the matrix {aij }, where i is the subscript for the row and j for the column. The i-th row of this matrix consists of the components of the new basis vector ei in terms of the old basis vectors. This matrix A is called the transformation matrix for going over from the orthonormal coordinate system R, with basis {e1 , e2 , e3 }, to the orthonormal system R with basis {e1 , e2 , e3 }. Two simple examples of transformation matrices are given below: 1.

The new frame R is the symmetric of R with respect to a plane perpendicular to axis Ox2 (Fig. 9.1a). In this case, the vectors e1 , e2 , e3 are given by e1 = e1 ,

e2 = −e2 ,

and the transformation matrix for ⎛ 1 A=⎝ 0 0

e3 = e3

this change of frame is given by ⎞ 0 0 −1 0 ⎠ . 0 1

Chapter 9 – Crystal anisotropy and tensors 2.

193

The new frame R is deduced from frame R through a rotation by angle ϕ around axis Ox2 (Fig. 9.1b). In this case, the vectors e1 , e2 , e3 are given by: e1 = cos ϕ e1 − sin ϕ e3 ,

e2 = e2 ,

and the transformation matrix for ⎛ cos ϕ A=⎝ 0 sin ϕ

e3 = sin ϕ e1 + cos ϕ e3

this change of frame is given by: ⎞ 0 − sin ϕ ⎠. 1 0 0 cos ϕ

x2

O M

x’3 x3

x 2 x’2

x’1 x1

O

x1

x3

x’1

x’3

x’2

(a)

(b)

Figure 9.1: Change in coordinate system. The new frame R (Ox 1 x 2 x 3 ), drawn in dotted lines, is obtained from the initial frame R (Ox 1 x 2 x 3 ), drawn in solid lines, through: (a) symmetry with respect to a plane M perpendicular to axis Ox 2 , (b) rotation by angle ϕ around axis Ox 2 .

9.3.3. Application to electrical conductivity In frame R {e1 , e2 , e3 }, the components jk of j can be written as a function of the components El of E: jk = σkl El . We want to express the coordinates ji of j in frame R as a function of the coordinates Ej of E in this frame. Using relations (9.8) and (9.9), we obtain: ji = aik jk = aik σkl El = aik σkl ajl Ej . E . Therefore The relation we want is ji = σij j = aik ajl σkl . σij

(9.12)

We note here for the last time that Einstein’s convention implies summing over the subscripts k and l which appear twice in the product.

194

Symmetry and Physical Properties of Crystals

Let x and y be two vectors with coordinates respectively xi and yi in basis {e1 ,e2 ,e3 }. Their coordinates xi and yi in basis {e1 , e2 , e3 } are given by xi = aik xk , yj = ajl yl . The product of two coordinates xi and yj takes the form xi yj = aik ajl xk yl , and a relation similar to that of Equation (9.12), connecting components σij σij . Thus, a coeﬃcient σij transforms in a change of axes like the product of two vector components.

9.4. Tensors 9.4.1. Deﬁnition of a tensor The last remark above allows us to understand the following deﬁnition of tensors: A tensor of rank n is (when three-dimensional space is considered) a set of 3n components, characterized by n subscripts, which transform in the change from one orthonormal frame to another orthonormal frame like the product of n vector components. For example, a tensor [T ] of rank 2 (also designated as a second-rank tensor), is a set of 9 coeﬃcients Tij deﬁned in an orthonormal frame R, and called the components of the tensor. In another orthonormal frame R , deduced from R through the transformation matrix {aij }, they become the components Tij such that Tij = aik ajl Tkl

(9.13a)

. Tij = aki alj Tkl

(9.13b)

and conversely:

The tensor as an entity is denoted by a letter, set between square brackets, e.g. [T ]. In the same way, a third-rank tensor [T ] has 27 components Tijk which transform in the same frame change according to relation = ail ajm akn Tlmn Tijk

(9.14a)

. Tijk = ali amj ank Tlmn

(9.14b)

and conversely:

Chapter 9 – Crystal anisotropy and tensors

195

Again in the same way, a fourth-rank tensor [T ] transforms in a change of frame according to = aim ajn akp alq Tmnpq Tijkl

(9.15a)

. Tijkl = ami anj apk aql Tmnpq

(9.15b)

and conversely:

We deduce immediately that a scalar is a tensor of rank 0 and that a vector is a tensor of rank 1. In practice, ascertaining the tensor character of a quantity deﬁned by 3n components implies checking that, in a change of frame, the components transform like the product of n components of vectors. The above deﬁnition restricts the general deﬁnition of tensors (see e.g. the books by Sands [2] or by Schwartz [3]) to the case of orthonormal frames.1 It makes the presentation of tensor physical properties of crystals much simpler while retaining the physics of the phenomena. In practice, problems of crystal physics are almost invariably treated with orthonormal frames.

9.4.2. An important property The derivation used to ﬁnd how the components of the electrical conductivity transform in a change of frame depends only on the vector nature of the quantities E and j and not on their physical nature. We can thus conclude that: If two vector physical quantities A and B, with components Ai and Bj in a given orthonormal axis system, are related by Bi = Tij Aj , then the physical quantity represented by the 9 coeﬃcients Tij is a tensor. With such a relation, we can state that Tij is a second-rank tensor [T ], and we can write B = [T ]A. We use the notation between square brackets to emphasize the tensor nature of the coeﬃcients Tij . More generally, it can be shown that A physical quantity relating a tensor physical quantity of rank p (which will be called the cause) to another tensor physical quantity of rank q (called the eﬀect) is represented by a tensor of rank n = p + q. Let us demonstrate this using an example. Suppose relation Ti = Uikl Vkl connects, in an orthonormal axis system (Ox1 x2 x3 ), tensor cause [V ], with rank 2, to tensor eﬀect T (a rank-one tensor, hence actually a vector) through the coeﬃcients Uikl . In another orthonormal axis system (Ox1 x2 x3 ), deduced from the former through the transformation 1. Using non-orthonormal axes requires the use of covariant and contravariant components, which we do not ﬁnd necessary here.

196

Symmetry and Physical Properties of Crystals

matrix {aij }, the components of T and [V ] are Ti and Vkl , related to the former ones through: = ami Ti , Tm

Vkl = ank apl Vnp

whence we deduce: = ami Ti = ami Uikl Vkl = ami Uikl ank apl Vnp Tm

so that = ami ank apl Uikl Vnp Tm = Umnp Vnp with Umnp = ami ank apl Uikl . This relation shows that Uikl is a tensor of rank 3 = 2+1.

The method we used applies whatever the ranks p and q of the cause and eﬀect tensors are. In what follows, we will frequently use this property to assert that a set of coeﬃcients indeed represents a tensor. We note that the relative electrical permittivity [ε] of a material is a secondrank tensor since it relates the induction D in the material to the electric ﬁeld E, i.e. D = ε0 [ε]E or Di = ε0 εij Ej where ε0 is the permittivity of vacuum.

9.4.3. Field tensors and material tensors Let us return to the example of electrical conductivity ji = σij Ej . This relation connects a cause, here the electric ﬁeld E, to an eﬀect, the current density j, through the electrical conductivity tensor [σ]. The electric ﬁeld E is an external action applied to the material, and it can be varied at will. It is a ﬁeld tensor. The same applies to the current density, which varies as E varies. On the other hand, the conductivity [σ] does not vary when the ﬁeld E varies. It characterizes a physical property of the crystal, the electrical conductivity: it is called a material tensor because it characterizes the material. Material tensors represent physical properties of the material. Their form largely depends on the isotropic or anisotropic character of the material. We saw, for example, that the electrical conductivity of a material becomes a scalar when the material is isotropic. Whatever their rank, the number of independent coeﬃcients necessary to deﬁne material tensors depends on the crystal symmetry of the material, as we will see in Sections 9.5.2 and 9.6.

Chapter 9 – Crystal anisotropy and tensors

197

In contrast, ﬁeld tensors are deﬁned in the same way for isotropic and anisotropic materials. We just saw the examples of the electric ﬁeld and of the electrical current density, which are rank-1 tensor. We will deﬁne in Chapter 11 the stress tensor and in Chapter 12 the strain tensor: they both are second-rank ﬁeld tensors. In Chapter 13, we will see that these two second-rank ﬁeld tensors are related, in a material, by a material tensor of rank 4 which caracterizes the elastic properties of the material.

9.5. Symmetry properties of tensors 9.5.1. Internal symmetry. Symmetric and antisymmetric tensors A tensor of rank n is symmetric with respect to two of its subscripts if the following relation applies: Tab...kl...n = Tab...lk...n . A tensor of rank n is antisymmetric with respect to two of its subscripts if the following relation applies: Tab...kl...n = − Tab...lk...n . Most material tensors have intrinsic symmetry (and, more rarely, antisymmetry) properties which result from thermodynamic considerations, independent of the nature of the crystal. They are called internal symmetry properties. On the other hand, some ﬁeld tensors also feature an internal symmetry, like the stress tensor whose symmetry is related to the balance condition for the solid to which it is applied (Sect. 11.4).

9.5.2. External symmetry of material tensors. Curie’s and Neumann’s principles The inﬂuence of crystal symmetry on material tensors can be described as a direct consequence of Curie’s principle. This principle was stated in 1894 by Pierre and Jacques Curie when studying piezoelectricity, which they had discovered in 1880. It is expressed as follows: When certain causes produce certain eﬀects, the symmetry elements of the causes must be present in the eﬀects. In the same way, when some eﬀects reveal some dissymetry, this dissymetry must be present in the causes which produce them. Consider once more an electric ﬁeld E applied to a material, and the current density j which results because of the electrical conductivity of the material [σ]: j = [σ]E. The causes here are the electric ﬁeld (a polar vector with symmetry ∞ m as shown by Fig. 9.2) and the crystal, with point group Gp (we saw in Sect. 9.2 that the group to be considered in discussing macroscopic properties is

198

Symmetry and Physical Properties of Crystals

the point group of the crystal). The eﬀect is the current density (a polar vector with symmetry ∞ m). Thus the symmetry of the causes is the intersection ∞ m ∩ Gp of the two point groups, which must be less than or equal to the symmetry of the current density ∞ m. The symmetry of the causes here depends on the symmetry of the crystal and on the orientation of the electric ﬁeld with respect to the symmetry elements of the crystal. In the most general case, when the electric ﬁeld has a general direction with respect to the symmetry elements of the crystal, there is no symmetry element common to the crystal and the electric ﬁeld. The symmetry ∞ m of the current density is then larger than the intersection ∞ m ∩ Gp , and nothing special can be stated. The interesting cases are those for which there is an intersection between ∞ m and Gp . For example, if Gp contains a q-fold axis and if the electric ﬁeld is parallel to the q-fold axis, then the intersection of the symmetry elements is the q-fold axis. The eﬀect, which must be at least as symmetric, will therefore be a current density parallel to the q-fold axis. Carrying this argument further, and using the properties of rank-2 tensors which we will see in the next chapter, precise information can be gained on the symmetry of the conductivity tensor in relation to the symmetry of the crystal. Curie’s principle is very general. It applies to all areas of physics. For crystallographic applications, one may prefer Neumann’s principle, which is less general and was laid down earlier (1885). It is expressed as follows: The symmetry elements of any macroscopic physical property of a crystal must include the symmetry elements of the point group of the crystal. Expressed diﬀerently, the symmetry group of any physical property of the crystal includes that of the crystal. Thus the point symmetry group of the crystal is either identical to the symmetry group of the physical property, or it is a subgroup of the latter. Consider for an illustration the example of pyroelectricity. Some crystals, called pyroelectrics (see Chap. 15), exhibit a spontaneous electric polarization P. This quantity is diﬃcult to evidence, because the distribution of electric charges which it entails are rapidly neutralized by free charges in air or by migration of charges within the crystal. However, since this polarization varies with temperature, a rapid variation of temperature ΔT entails a rapid variation, ΔP, of the polarization, which in turns produces a current which is easy to detect. ΔP and ΔT are related by: ΔP = pΔT where p is a vector (rank-1 tensor) which represents the property of pyroelectricity in the material. The symmetry group of a polar vector is ∞ m (Fig. 9.2). Therefore, according to Neumann’s principle, the point group of a pyroelectric crystal must be a subgroup of this group. The only possibilities are the groups: 1

2

3

4

6

Chapter 9 – Crystal anisotropy and tensors

199

A

M

Figure 9.2: Symmetry elements of a polar vector: an A∞ axis parallel to the vector, and an inﬁnity of mirrors containing this axis and those obtained by adding to each of these groups a mirror that goes through the n-fold axis, hence the groups m

mm2

3m

4mm

6mm

thus in total 10 point groups. Crystals with one of these 10 point groups can feature pyroelectricity. It is clear that, if the crystal belongs to one of these groups, the spontaneous polarization will be parallel to axis An for all the groups that have one. For group m, it will be parallel to the mirror and for group 1, its direction is not predetermined by symmetry. We just applied Neumann’s principle directly to a vector physical property for which the symmetry (∞ m) is known. It can also be applied to a symmetric second-rank tensor, whose symmetry is that of an ellipsoid, mmm, as we will see in Section 10.5. For higher-rank tensors, it is convenient to use an equivalent form of Neumann’s principle: if a crystal is invariant under a given symmetry operation, all of its physical properties are invariant under this symmetry operation. Imagine the following experiment. We ﬁrst measure a physical property in a given reference system for a given position of the crystal. Then we submit the crystal to one of its point symmetry operations, and we again measure the physical property in the same reference system. The result obtained must be identical to the former one. Since it is equivalent to perform the symmetry operation on the crystal or the inverse operation (necessarily also a member of the group) on the coordinate system, we will retain the second deﬁnition. Thus: To determine the number of independent components of a tensor representing a physical property of a given crystal, it is suﬃcient to express the invariance of the tensor when all the symmetry operations of the crystal’s point group are applied to the coordinate system.

200

Symmetry and Physical Properties of Crystals

It is clearly suﬃcient to consider only those symmetry operations which are generating all the elements of the point group.

9.6. Reduction in the number of independent coeﬃcients of a material tensor We present two methods for reducing the number of components of a tensor, both using the invariance property stated above.

9.6.1. Method using the transformation matrix We apply the very deﬁnition of a tensor based on the transformation of its components in a change of reference frame (Sect. 9.4.1), viz. = ail ajm akn . . .Tlmn... Tijk...

The Tijk... are the coeﬃcients of a tensor expressed in a ﬁrst, general, orthonor are the coeﬃcients of this same tensor expressed in mal frame and the Tijk... another frame, deduced from the former by a symmetry operation of the crystal’s point group. The aij are the coeﬃcients of the transformation matrix from the ﬁrst frame to the second. The invariance of the components of the tensor under this special change in frame implies that = Tijk.... Tijk...

As an example, we consider a physical property represented by a secondrank tensor, and examine in turn the case of crystals with point groups 2, m and 2/m. If the point group is 2, we can choose the axis system so that axis Ox2 is parallel to the two-fold axis. A rotation by π around axis Ox2 changes the frame R {e1 , e2 , e3 } into a frame R {e1 , e2 , e3 } such that e1 = −e1 ,

e2 = e2 ,

e3 = −e3 .

The only non-zero coeﬃcients of the frame change matrix A are thus: a11 = −1,

a22 = 1

and

a33 = −1

and we deduce that in this transformation = T11 T11 T12 T21

= −T12 = −T21

T22 = T22 T13 T31

= T13 = T31

T33 = T33

T23 = −T23

T32 = −T32 .

(9.16)

Furthermore, we must have Tij = Tij .

(9.17)

Chapter 9 – Crystal anisotropy and tensors

201

= −T We thus deduce for instance that T12 = 0 since T12 12 from (9.16) and T12 = T12 from (9.17). In the same way, T21 = 0, T23 = 0 and T32 = 0, and the tensor ﬁnally is: ⎛ ⎞ T11 0 T13 ⎝ 0 T22 0 ⎠ (9.18) T31 0 T33

For this representation of the tensor, we use the classical notation of matrices: the ﬁrst subscript designates the row and the second one the column. If the point group is m, we can choose an axis system such that axis Ox2 is perpendicular to the mirror. This mirror operation changes frame R into a frame R such that e1 = e1

e2 = −e2

e3 = e3 .

The non-zero coeﬃcients in the transformation matrix are thus a11 = 1, a22 = −1 and a33 = 1. We easily see that we obtain the same tensor form as above in (9.18). Thus the presence of a two-fold axis or of a mirror perpendicular to this axis reduces the number of components of a second-rank tensor in the same way. The form given in (9.18) is therefore that for a second-rank tensor representing a physical property of a crystal belonging to any one of the point groups 2, m, 2/m (monoclinic groups) when the axis Ox2 is chosen parallel to the 2-fold axis or perpendicular to the mirror.

9.6.2. “Direct inspection” method This method, due to Fumi [4], uses another aspect of the deﬁnition of tensors, viz. the fact that the components of a tensor transform in an axis change like a product of coordinates. We thus consider directly the products of coordinates. Let us apply this method to the example above. A rotation by π of the coordinate system around axis Ox2 changes the coordinates xi of a point M into coordinates xj such that x1 = −x1 ,

x2 = x2 ,

x3 = −x3 .

We immediately deduce that, for a second-rank tensor, only the components that have one subscript, and only one, equal to 2 will be zero since, in these cases, xi xj = −xi xj , whence Tij = −Tij while Tij = Tij . In the same way, the operation of a mirror perpendicular to Ox2 changes the coordinates xi of a point M into coordinates xj such that x1 = x1 ,

x2 = −x2 ,

We thus retrieve the preceding results.

x3 = x3 .

202

Symmetry and Physical Properties of Crystals

This method is easy to apply, and it is the one used in practice for all the symmetry operations for which the new components xi are expressed as functions of a single component xi . This is the case for all symmetry operations associated to 2- and 4-fold axes, to centers of symmetry and to mirrors. For 3and 6-fold axes, the preceding method, using the transformation matrix from one frame to another, is preferred, except for cubic crystals, where the 3-fold axes are parallel to the < 111 > directions. In the latter case, one chooses an orthonormal coordinate system parallel to the basis vectors of the crystal system. A rotation of the coordinate system by 2π/3 around a [111] direction transforms the coordinates xi of a point P into coordinates xi such that x1 = x2 ,

x2 = x3 ,

x3 = x1

and the direct inspection method is easy to use. We note that, in all cases, the reduction in the number of components is performed with an orthonormal axis system in which one axis (or several) is parallel or perpendicular to a symmetry element of the crystal.

9.6.3. Special case: central symmetry (inversion symmetry) In this case both methods are equally convenient. The transformation matrix is such that aij = −δij , and we obtain, for a rank-n tensor = (−1)n Tijk... = Tijk... Tijk...

(9.19)

1.

If n is odd, we conclude that all the tensor’s components are zero. Thus an odd-rank tensor representing a physical property of a crystal has non-zero components only if the crystal has no center of symmetry. We will see that piezoelectricity, which is described by a third-rank tensor, exists only in crystals that do not have a center of symmetry.

2.

If n is even, the tensor is unchanged by the existence of a center of symmetry, and adding a center of symmetry changes nothing to the number of independent coeﬃcients of the tensor. Hence, for the physical properties represented by even-rank tensors, the number of independent coeﬃcients is the same for all point groups of a Laue class (see Sect. 5.7).

We note that relation (9.19) applied to even-rank tensors shows that a central symmetry operation applied to the coordinate system in which the tensor components are expressed leaves its components invariant. This property can be considered without any reference to a crystal. It is general, and the property obtained is therefore also valid for ﬁeld tensors. We can thus state this result in the following form: a central symmetry operation applied to any even-rank tensor (be it a ﬁeld tensor or a material tensor) leaves this tensor invariant.

Chapter 9 – Crystal anisotropy and tensors

203

9.7. Exercises Exercise 9.1 Consider a symmetrical rank-2 material tensor [T ] representing a physical property of a crystal with point group 3. Let Tij be the components of this tensor in an orthonormal axis system (Ox1 x2 x3 ) where Ox3 is parallel to the 3-fold axis. 1.

Let (Ox1 x2 x3 ) be an axis system deduced from (Ox1 x2 x3 ) through a rotation by 2π/3 around axis Ox3 . Determine the transformation matrix {aij } from axis system (Ox1 x2 x3 ) to axis system (Ox1 x2 x3 ).

2.

, T and T of [T ] in the axis system (Ox x x ), Express the components T11 12 22 1 2 3 and deduce that T11 = T22 and T12 = 0.

3.

, T and T , and show that T Calculate T13 13 = T23 = 0 and T33 = 0. 23 33

Exercise 9.2 Use the direct inspection method to determine the number of non-zero coefﬁcients for a material rank-2 tensor of a crystal with point group mmm if its components are expressed in a frame with axes perpendicular to the mirrors.

204

Symmetry and Physical Properties of Crystals

References [1] J.L. Spain, in Chemistry and Physics of Carbon, vol. 8, ed. by P.L. Walker (Marcel Dekker Publisher, New York, 1973), pp. 130–131 [2] D.E. Sands, Vectors and Tensors in Crystallography (Dover Publications, Mineola, New York, 1995) [3] L. Schwartz, Les tenseurs (Hermann, Paris, 1975) [4] F.G. Fumi, Physical properties of crystals: the direct inspection method, Acta Crystallographica 5, 44–48 (1952)

Chapter 10

Second-rank tensors This chapter is devoted to the study of the characteristic properties of symmetric tensors of rank 2. They represent many physical properties which, in isotropic materials, are described by a simple scalar. The end of this chapter introduces axial vectors, which are antisymmetric tensors of rank 2, and gives examples.

10.1. Introduction Second-rank tensors are very important in physics. Because most of them are symmetric, it is useful to investigate their special properties, and in particular the quadric which is associated to them (Sect. 10.2, 10.3 and 10.4). Section 10.5 investigates the eﬀect of crystal symmetry on material tensors of rank 2. Section 10.6 deﬁnes axial vectors, and shows that they are antisymmetric tensors of rank 2.

10.1.1. Symmetric and antisymmetric tensors A second-rank tensor is symmetric if Tij = Tji whatever i and j, and the matrix which represents it in a general axis system has the form ⎞ ⎛ T11 T12 T13 ⎝ T12 T22 T23 ⎠ . T13 T23 T33 There are thus 6 independent coeﬃcients. A second-rank tensor is antisymmetric if Tij = −Tji , hence T11 = T22 = T33 = 0, so that, in matrix representation: ⎞ ⎛ 0 T12 T13 ⎝ −T12 0 T23 ⎠ . −T13 −T23 0 There are thus 3 independent coeﬃcients.

© Springer Science+Business Media Dordrecht 2014 C. Malgrange et al., Symmetry and Physical Properties of Crystals, DOI 10.1007/978-94-017-8993-6_10

205

206

Symmetry and Physical Properties of Crystals

Any second-rank tensor [T ] can be written as the sum of a symmetric tensor [S] and an antisymmetric tensor [A]: [T ] = [S] + [A], with Tij + Tji 2 Tij − Tji . Aij = 2 Sij =

and

This decomposition is independent of the frame in which tensor [T ] is expressed. We demonstrate this for the symmetric part. In another orthonormal axis of tensor [S] become S = a a S system (Ox1 x2 x3 ), the components Sij ik jl kl ij = S . (Eq. (9.13a)). If Skl = Slk , it is clear that Sij ji

10.1.2. Matrix form of second-rank tensors We saw that it is customary to represent the components of a rank-2 tensor, in a given system of axes, by a matrix, extending to tensors the usual rule for writing matrices. Thus the component Tkl of the tensor is at the intersection of the k-th row and the l-th column of matrix T . In another system of axes, deduced from the ﬁrst one through the transformation matrix A, the new takes the form component Tkl = aki alj Tij . Tkl

If AT is the transposed matrix of A, aTij = aji and = aki Tij aTjl Tkl

so that, in matrix notation T = AT AT .

(10.1)

10.1.3. Trace The trace of a second-rank tensor [T ], represented in a given system of axes, is deﬁned by: Tr [T ] = T11 + T22 + T33 = Tii . It is independent of the referential chosen to represent the tensor. The trace of tensor [T ] in a new axis system, Tr ([T ]) , is expressed, using relation (9.13a), by: (Tr [T ]) = Tii = aik ail Tkl . From (9.10): aik ail = δkl and (Tr [T ]) = δkl Tkl = Tkk . Hence (Tr [T ]) = Tr [T ].

Chapter 10 – Second-rank tensors

207

10.2. Representative quadric for a symmetric rank-2 tensor 10.2.1. Characteristic surface Consider the following equation: Sij xi xj = ±1 = ε

(10.2)

where, for the moment, the coeﬃcients Sij are general, but satisfy the condition Sij = Sji . When expanded, this equation takes the form S11 x21 + S22 x22 + S33 x23 + 2S12 x1 x2 + 2S13 x1 x3 + 2S23 x2 x3 = ε.

(10.3)

The locus of the points M with coordinates x1 , x2 , x3 in an orthonormal frame is a second-degree surface, also called quadric (Q) (an ellipsoid or a hyperboloid), having for its center the coordinate origin O. We want the equation of this quadric in another frame (Ox1 x2 x3 ) obtained from (Ox1 x2 x3 ) through the transformation matrix A = {aij }. xi = aki xk

From Equation (9.9): and Equation (10.2) becomes:

Sij aki xk alj xl = ε x x = ε if S = a a S . which can be written as: Skl ki lj ij k l kl

Thus the coeﬃcients Sij which deﬁne the quadric (Q) transform in a change of orthonormal frame like the components of a second-rank tensor. If the coeﬃcients Sij in Equation (10.2) are the coeﬃcients of a symmetric tensor, the quadric (Q) is a geometrical representation of this tensor. We have thus deﬁned the representation quadric of a symmetric tensor [S].

10.2.2. Principal axes and principal coeﬃcients The quadrics (ellipsoids or hyperboloids on Fig. 10.1) have as symmetry elements three mutually perpendicular mirrors, three 2-fold axes at the intersections of these mirrors, and a center of symmetry. In an orthonormal set of axes (Ox1 x2 x3 ) parallel to these 2-fold axes, called the principal axes of the quadric, the equation of the quadric becomes: (x1 )2 + S22 (x2 )2 + S33 (x3 )2 = ε. S11

(10.4)

In this new system of axes, called the principal axes of the tensor, the tensor takes a diagonal form: ⎞ ⎛ 0 S11 0 ⎝ 0 S22 0 ⎠ 0 0 S33

208

Symmetry and Physical Properties of Crystals x3

x3

x2 x1

(a)

(b)

x3

x3

(c)

(d)

Figure 10.1: Representation quadrics of a symmetric second-rank tensor: (a) an ellipsoid, if the three principal values have the same sign; (b) onesheeted hyperboloid; (c) two-sheeted hyperboloid; (d) the set of two hyperboloids representing the tensor when one of the principal values has a sign opposite to the two others , S and S are called the principal values or the principal coeﬃcients and S11 22 33 of tensor [S].

To determine these principal axes (of the quadric and of the tensor), we note that, along these special directions, the normal to the quadric is parallel to the radius vector of the quadric. We know that, if the equation of a surface is f (x1 , x2 , x3 ) = 0, the components Xi of a vector perpendicular to this surface are Xi = ∂f /∂xi . A vector normal to the quadric with Equation (10.3) thus has for its components Xi at a point with coordinates xj : Xi = 2Sij xj . It is parallel to the radius vector with components xi if: Sij xj = λxi

(10.5)

Chapter 10 – Second-rank tensors

209

where λ is any scalar. This system of three equations is just the tool needed to determine the eigenvectors and eigenvalues of matrix {Sij }. Since this matrix is real and symmetric, it has three real and orthogonal eigenvectors, the eigenvalues of which are real. We can thus determine the directions of the symmetry axes of the quadric; they coincide with the principal axes of the tensor.

10.2.3. Shape of the quadric In the frame (Ox1 x2 x3 ) of its principal axes, the quadric is deﬁned by the three , S and S . Its geometrical shape depends on the signs of coeﬃcients S11 22 33 these three coeﬃcients. , S and S are positive, we choose ε = 1, and the equation of the If S11 22 33 quadric can be expressed in the form:

x12 x22 x32 + 2 + 2 = 1, a2 b c the equation of an ellipsoid (Fig. 10.1a) with semi-axes a, b and c such that: 1 b= , S22

1 a= , S11

1 c= . S33

The principal values of the tensor are thus the reciprocals of the squares of the semi-axes of the ellipsoid. , S and S are negative, the associated quadric would be an imaginary If S11 22 33 ellipsoid if ε was chosen as equal to 1. We choose ε = −1 so that the quadric is an ellipsoid. The principal values of the tensor are negative, and their absolute values are the reciprocals of the squares of the semi-axes of the ellipsoid. < 0), If two coeﬃcients are positive and the third one negative (for example S33 and if we choose ε = 1, the equation of the quadric has the form:

x12 x22 x32 + 2 − 2 = 1, a2 b c with a2 =

1 , S11

b2 =

1 , S22

c2 = −

1 . S33

This is the equation of a one-sheet hyperboloid (Fig. 10.1b). The sections of this hyperboloid by the planes x3 = const are ellipses, while the sections by the planes x1 = const and x2 = const are hyperbolas. If we choose ε = −1, the equation becomes:

−

x12 x22 x32 − 2 + 2 =1 a2 b c

and the quadric is a two-sheeted hyperboloid (Fig. 10.1c). In order to obtain a representation of the tensor in all directions of space, the representation

210

Symmetry and Physical Properties of Crystals

quadric of the tensor consists of the two hyperboloids tangent to the same cone, whose apex is the origin of the axes (Fig. 10.1d). > 0), If two coeﬃcients are negative and the third one positive (for example S33 we retrieve the preceding case if we set:

a2 = −

1 , S11

b2 = −

1 , S22

c2 =

1 . S33

The one-sheet hyperboloid is obtained with ε = −1 and the two-sheeted one with ε = 1. We will see an application in Section 12.6. In practice, the principal values of a tensor are usually all positive, and the quadric is then an ellipsoid, the equation of which is given by (10.4) with ε = 1. This is, for simplicity, what we will assume in the next section.

10.3. Properties of the quadric Consider a second-rank tensor [T ] which relates vector A to vector B through relation B = [T ]A, i.e. Bi = Tij Aj . We will, to simplify the presentation, call vector A the cause and vector B the eﬀect even if tensor [T ] is a ﬁeld tensor for which this denomination is not justiﬁed.

10.3.1. Normal to the quadric We saw (Eq. (10.5)) that the normal to point M (x1 , x2 , x3 ) of the quadric Tij xi xj = 1 is a vector with components Xi = 2Tij xj , i.e. a vector parallel to the vector [T ]OM with components Tij xj . We deduce that, if the cause vector is parallel to radius vector OM, the associated eﬀect vector is parallel to the normal to the quadric at point M. Figure 10.2 illustrates this result. We chose the electric ﬁeld E as the cause vector, and its eﬀect is the current density j, which is related to it by the electrical conductivity [σ]: j = [σ]E. x2

j E s

O

M x1

Figure 10.2: If the direction of the cause vector (electric ﬁeld E) is along OM, the eﬀect vector (electric current density j) is along the normal at point M to the quadric representing the electrical conductivity tensor.

Chapter 10 – Second-rank tensors

211

10.3.2. Length and physical meaning of the radius vector Let M be a point of the quadric representing tensor [T ] which connects cause vector A to eﬀect vector B through relation B = [T ]A. Set: OM = rs where s is a unit vector. We deduce: xi = rsi . The equation of quadric Tij xi xj = 1 becomes: Tij r 2 si sj = 1 so that

1 = si Tij sj r2

which can be written in matrix form: ⎛ ⎞⎛ ⎞ T11 T12 T13 s1 1 = s1 s2 s3 ⎝ T12 T22 T23 ⎠ ⎝ s2 ⎠ . r2 T13 T23 T33 s3

(10.6)

(10.7)

If the cause vector A, with norm A, is parallel to OM, we have A = As, i.e. Aj = Asj . The components Bi of the eﬀect vector are given by: Bi = Tij Aj = Tij sj A and the component of B parallel to A, i.e. B · s, becomes:

1 B · s = Bi si = si Tij sj A = A 2 . r

(10.8)

We deduce that, for a cause vector with unit norm (A = 1), parallel to a given radius vector of the quadric, the reciprocal of the square of the length of this radius vector is equal to the projection of the corresponding eﬀect vector on the direction of the cause vector.

10.3.3. Intensity of a physical property in a given direction If tensor Tij is a material tensor representing a given physical property, si sj Tij represents the value of this physical quantity in direction s. We demonstrate this by taking the example of electrical conductivity [σ], with components σij in a given axis system. A measurement of the conductivity of a crystal can be performed by using a parallel-faced plate of this crystal, with thickness e small with respect to the sides of the main face. A voltage V is applied between the metallized major faces. It induces, except for edge eﬀects which we neglect, an electric ﬁeld E perpendicular to the plate, so that E = Es where s is a unit

212

Symmetry and Physical Properties of Crystals

vector perpendicular to the plate and E = V /e. We then measure the intensity in the circuit, and deduce the current density (the intensity of the current in the circuit, divided by the area of the crystal perpendicular to the electric ﬁeld, hence in this case the area of the major faces). The latter is the component js of the current density along the normal s to the crystal (Fig. 10.3), so that: js = j · s = ji si = σij sj si E.

j

s

js

E

V

Figure 10.3: Schematic diagram of the principle of the experimental device for measuring the electrical conductivity of a crystal plate, the major faces of which were metallized The conductivity in direction s is deﬁned as the quantity σs such that: σs =

js = σij si sj . E

In a general way, the value Ts in a direction with unit vector s of a physical property represented by tensor [T ] is given by si sj Tij . From (10.6), Ts =

and

1 r2

1 r= √ . Ts

(10.9)

Knowing the length of the radius vector OM of the quadric thus provides the value of the physical property in direction OM.

Chapter 10 – Second-rank tensors

213

10.4. Geometrical determination of the principal axes and principal coeﬃcients: the Mohr circle construction We just saw that a symmetric tensor [T ] its principal axes (Ox1 x2 x3 ): ⎛ T11 0 T = ⎝ 0 T22 0 0

can be written in the referential of ⎞ 0 0 ⎠. T33

Consider a new axis system (Ox1 x2 x3 ) deduced from (Ox1 x2 x3 ) through rotation by angle θ around Ox3 . In this new axis system, the components Tij of [T ] are expressed as: Tij = aik ajl Tkl where the transformation matrix A = {aij } is: ⎛ ⎞ cos θ sin θ 0 A = ⎝ − sin θ cos θ 0⎠ . 0 0 1 We obtain:

= a1k a1l Tkl = a11 a11 T11 + a12 a12 T22 + a13 a13 T33 , T11 = cos2 θ T11 + sin2 θ T22 , T11

T22 = a2k a2l Tkl = a21 a21 T11 + a22 a22 T22 + a23 a23 T33 ,

= sin2 θ T11 + cos2 θ T22 , T22 = T33 . T33

In the same way:

= 0, T13

= 0, T32

= T21 = − sin θ cos θ T11 + sin θ cos θ T22 . T12

Thus, tensor [T ] is expressed, in the frame (Ox1 x2 x3 ), as: ⎞ ⎛ 0 T11 T12 ⎝ T12 T22 0 ⎠. 0 0 T33 , T and T as a function of cos 2θ and sin 2θ: We now express T11 22 12

1 1 (T11 + T22 ) − (T22 − T11 ) cos 2θ 2 2 1 1 = (T11 + T22 ) + (T22 − T11 ) cos 2θ 2 2 1 = (T22 − T11 ) sin 2θ. 2

= T11 T22 T12

(10.10)

214

Symmetry and Physical Properties of Crystals

The set of relations (10.10) can be expressed graphically by using the Mohr circle representation (Fig. 10.4). Points A and B are placed along axis Ox1 so that OA = T11 and OB = T22 . We draw circle C, with its center C at the middle of segment AB, and with diameter d equal to the norm of AB. Relations (10.10) become: AB cos 2θ, 2 AB cos 2θ, = OC + 2 AB = sin 2θ. 2

= OC − T11 T22 T12

We draw the axis Cx2 such that angle (Cx1 , Cx2 ) is equal to π/2, then the radius CP of circle C enclosing angle 2θ with axis Ox1 . Let P be the point diametrically opposite to P. Let H and J be the respective projections of P and = OH, P on axis Cx1 , and K the projection of P on axis Cx2 . We see that: T11 T22 = OJ and T12 = CK. x2

C

O

T11 A

T’11 H

T’12 K

P 2 T’22

C

J

T22 B

x1

P’

Figure 10.4: Mohr circle construction This construction makes it possible to easily determine how the tensor coeﬃcients vary when the coordinate axes are rotated. Furthermore, this construction, when performed the other way, makes it possible to quickly determine the principal axes of a second-rank tensor for which only one principal axis is known. The procedure that provides the principal axes and principal values of a tensor which, expressed in its initial frame, has the form: ⎛ ⎞ T11 T12 0 ⎝ T12 T22 0 ⎠ 0 0 T33

Chapter 10 – Second-rank tensors

215

is given below, where ψ is the angle by which we must rotate the initial frame around axis Ox3 to obtain the diagonal form (the angle opposite to the preceding angle θ), and T11 and T22 are the principal values associated to axes Ox1 and Ox2 respectively. and OJ = T . Let Points H and J are placed on axis Ox1 so that OH = T11 22 C be the middle of HJ. Point K is placed on axis Cx2 , perpendicular to Ox1 , . Points J and K deﬁne respectively the abscissa and the so that CK = T12 ordinate of a point P in the axis system (Cx1 , Cx2 ). Angle 2ψ is then the angle (CP, Cx1 ). Let R be the length of vector CP. We obtain T11 = OC − R and T22 = OC + R.

Notes: 1.

It is evident that, if angle 2ψ is larger than π, it will be simpler to choose an angle equal to 2ψ − π, i.e. a rotation angle ψ − π/2, and to interchange T11 and T22 .

2.

If the subspace to be diagonalized is (Ox1 , Ox3 ), then axis Ox1 will be substituted by Ox3 and axis Ox2 by Ox1 in the above construction.

10.5. Eﬀect of crystal symmetry To determine the number of independent coeﬃcients of a symmetric secondrank material tensor (a tensor representing a physical property of a crystal), we can use either of the methods presented in Sections 9.6.1 and 9.6.2. A more elegant and quicker method consists in using the representative quadric of the tensor: according to Neumann’s principle, it must be at least as symmetric as the crystal. The symmetry elements of a general quadric are: one symmetry center, three A2 axes, which are the principal axes, three mirrors perpendicular to the A2 axes. Hence the point group of the quadric is mmm. We deduce for example that: if the crystal has a 2-fold axis, one of the principal axes of the quadric is necessarily parallel to this 2-fold axis. if the crystal has an axis with order n larger than 2 (n = 3, 4 or 6), the quadric must also have an axis with order larger than 2. For a quadric, this can only be an axis of revolution (the symmetry of a revolution quadric is ∞/mm). This axis of revolution is then parallel to the n-fold axis.

216

Symmetry and Physical Properties of Crystals

We now apply these results to the various crystal groups, assuming for simplicity that the representation quadric of the tensor is an ellipsoid. This assumption does not aﬀect the generality of the results to be obtained. We will also see that, ﬁnally, the number of independent coeﬃcients of a symmetric second-rank tensor is the same for all the groups of a given crystal system.

10.5.1. Triclinic system A crystal with point group 1 has no symmetry element. The directions of the principal axes of the quadric then have no special connection with those of the basis vectors a, b and c of the crystal. The tensor representing the physical property of this crystal then has 6 independent coeﬃcients. If the point group of the crystal is ¯1, the result is the same since the quadric has a center of symmetry. This result is no surprise since we showed (Sect. 9.6.3) that even-rank tensors are invariant under a central symmetry operation. The tensor has the most general form: ⎞ ⎛ T11 T12 T13 ⎝ T12 T22 T23 ⎠ . T13 T23 T33 Its principal axes can now be determined. The six independent coeﬃcients are retrieved: the three principal values, and the three parameters which deﬁne the orientation, with respect to the crystal itself, i.e. with respect to the basis vectors of its unit cell, of the orthonormal trihedron parallel to the principal axes.

10.5.2. Monoclinic system Such a crystal has at least a 2-fold axis (group 2) or a mirror (group m). One of these symmetry elements therefore necessarily coincides with one of the symmetry elements of the ellipsoid. If an orthonormal axis system is chosen so that axis Ox3 be parallel to axis A2 , or perpendicular to mirror m, the tensor takes the form: ⎞ ⎛ T11 T12 0 ⎝ T12 T22 0 ⎠ . 0 0 T33 If the crystal group is 2/m, the same result is obtained, since the quadric has a mirror perpendicular to each of the A2 axes. We retrieve the result of the example discussed in Section 9.6.1, except that we here chose axis Ox3 parallel to the 2-fold axis and perpendicular to the mirror.

10.5.3. Orthorhombic system In this system, a crystal has at least three mutually orthogonal 2-fold axes (group 222) or two mutually orthogonal mirrors (group mm2). These symme-

Chapter 10 – Second-rank tensors

217

try elements must be common to the crystal and to the ellipsoid representing the physical property. The axes of the ellipsoid are therefore parallel to the basis vectors of the orthorhombic unit cell: thus the orientation of the ellipsoid is ﬁxed. In a system of orthonormal axes parallel to the basis vectors a, b and c, the tensor has the form: ⎛ ⎞ T11 0 0 ⎝ 0 T22 0 ⎠ . 0 0 T33 This result is valid also for group mmm, which is the symmetry group of the ellipsoid.

10.5.4. Uniaxial systems: rhombohedral, trigonal and hexagonal A crystal belonging to any one of these systems has at least one n-fold axis, with n larger than 2 (except for groups ¯4 and ¯ 42m). The same must apply to the ellipsoid, which is therefore of revolution around this axis. If Ox3 is chosen parallel to axis An , the tensor has the form: ⎞ ⎛ 0 T11 0 ⎝ 0 T11 0 ⎠ . 0 0 T33 The additional symmetry elements in any of these crystal groups do not contribute additional relations among the coeﬃcients, because the ellipsoid already has all the symmetry elements which can be added. The same result is obtained for groups ¯4 and ¯42m, for example using the direct inspection method (Exercise 10.4) or, alternatively, by noting that the number of independent coeﬃcients for even-rank material tensors is the same for all groups in a given Laue class (Sect. 9.6.3).

10.5.5. Cubic system All groups in this crystal system have four A3 axes. The only ellipsoid compatible with the presence of four A3 axes is a sphere. The quadric is therefore a sphere. The tensor is diagonal, with its three coeﬃcients equal: ⎛ ⎞ T 0 0 ⎝ 0 T 0 ⎠ 0 0 T whatever the axis system in which it is represented. We conclude that: The physical properties represented by a rank-2 tensor are isotropic in a cubic crystal.

218

Symmetry and Physical Properties of Crystals

10.6. Axial vectors, or antisymmetric rank-2 tensors 10.6.1. Polar vectors, axial vectors Two families of vector-type physical quantities must be distinguished: the quantities obviously represented by vectors (displacement, velocity, acceleration, force. . . ): these are called polar vectors. the quantities which describe a rotation, such as angular velocity, the moment of a force, magnetic ﬁeld. . . These are called axial vectors.

They are denoted as V and represented by a line and a sense of rotation around this line. It is however convenient to also represent them through vectors. This requires choosing a convention to connect the direction of the vector and the sense of rotation. The convention chosen is the following: the vector points so that the rotation associated to the axial vector be, for this vector, in the direct direction (Fig. 10.5).

Figure 10.5: Convention for representing axial vectors through vectors These two vector families transform diﬀerently under some symmetry operations. If an axial vector is submitted to a rotation, the sense of rotation of the axial vector is conserved. Therefore a polar vector and an axial vector transform the same way in a rotation operation. In contrast, the behavior is diﬀerent for symmetry with respect to a center and with respect to a plane. Consider a given vector OP, representing ﬁrst a polar vector, and then an axial vector, using the above convention. Let x1 , x2 and x3 be the components of vector OP in a given orthonormal axis system, and let x1 , x2 and x3 be those of vector OP , the transform of OP in the symmetry operation. Consider ﬁrst the operation corresponding to symmetry with respect to plane (Ox1 , Ox2 ). The components of the polar vector OP are (Fig. 10.6a): x1 = x1 ,

x2 = x2 ,

x3 = −x3 .

Those of the axial vector OP are (Fig. 10.6b and c): x1 = −x1 ,

x2 = −x2 ,

x3 = x3 .

Now consider the operation corresponding to symmetry with respect to point O. The components of the polar vector OP are (Fig. 10.7a): x1 = −x1 ,

x2 = −x2 ,

x3 = −x3 .

Chapter 10 – Second-rank tensors

219 x3

P

O

x2

x1

(a)

P’

x3

x3

P’

P

O x2

x1

x1

(b)

x2

O

(c)

Figure 10.6: Transformation of polar and axial vectors through symmetry with respect to plane (Ox 1 , Ox 2 ): (a) polar vector; (b) axial vector; (c) polar vectors associated to the axial vectors of Figure (b) x3

P

O x2

x1

(a) x3

x3 P P’

O x2

x1

(b)

x1

O

x2

(c)

Figure 10.7: Transformation of polar and axial vectors through symmetry with respect to point O: (a) polar vector; (b) axial vector; (c) polar vectors associated to the axial vectors of Figure (b)

220

Symmetry and Physical Properties of Crystals

and those of the axial vector OP are (Fig. 10.7b and c) x1 = x1 ,

x2 = x2 ,

x3 = x3 .

The polar and axial vectors thus transform the same way in direct isometries (rotation), and diﬀerently in indirect isometries (symmetry with respect to a plane and central symmetry). This diﬀerence is also encountered when performing a change in coordinate system, since transforming a vector through a symmetry operation is equivalent to performing the inverse symmetry operation on the coordinate system. In a rotation of the coordinate system (direct isometry), the components of a polar vector and of an axial vector transform the same way: from relation (9.8): xi = aij xj

(10.11)

where the xi are the old components, the xi the new components and {aij } is the transformation matrix for going from the old coordinate system to the new system. In contrast, if the coordinate system is submitted to a symmetry with respect to a plane or a central symmetry, which are indirect isometries, it can be checked that the new components xi of the axial vector are expressed as a function of the old ones xi through relation: xi = −aij xj .

(10.12)

Further, since the determinant Δ of matrix {aij } is equal to +1 for direct symmetry operations and to −1 for indirect symmetry operations, we can, for axial vectors, collect relations (10.11) and (10.12) into a single relation: xi = Δaij xj

(10.13)

where Δ is the determinant of the transformation matrix from the old to the new system.

10.6.2. Example of an axial vector: the cross product

Consider a cross product: W = P×Q where P and Q are two polar vectors. It is an axial vector because it is related to the sense of rotation of vector P toward vector Q. It can in fact easily be checked that a central symmetry operation on vectors P and Q transforms vector W into itself. Let p1 , p2 , p3 and q1 , q2 , q3 be the components of P and Q respectively, in an orthonormal axis system (Ox1 x2 x3 ). The components wi of the cross product W = P × Q are:

w1 = p 2 q 3 − p 3 q 2 w2 = p 3 q 1 − p 1 q 3 w3 = p 1 q 2 − p 2 q 1

(10.14)

Chapter 10 – Second-rank tensors

221

which can be written in a condensed form which will prove useful later on: wk = δkij pi qj .

(10.15)

δijk is the Levi-Civita symbol, deﬁned, for any axis

system,1

as:

δijk = 0 if at least two of the subscripts i, j and k are equal, δijk = 1 if the permutation ijk is direct (123, 231, 312), δijk = −1 if it is inverse (132, 213, 321).

Let w1 , w2 , w3 be the components of vector W , the transform of W in a symmetry with respect to the origin. Since a central symmetry changes P into −P and Q into −Q, we immediately see on Equations (10.14) that w1 = w1 , w2 = w2 and w3 = w3 , so that W = W. We can associate the components of W to coeﬃcients Vij deﬁned by:

Vij = pi qj − qi pj for i = j V11 = V22 = V33 = 0.

and

w1 = V23 = −V32 ,

We thus have

w2 = V31 = −V13 ,

(10.16)

w3 = V12 = −V21 . In another axis system (Ox1 x2 x3 ), deduced from the preceding one through the transformation matrix A with coeﬃcients aij , the components of vectors P and Q become: pi = aij pj

and

qi = aij qj .

The coeﬃcients Vij become, in this new axis system, Vij such that: Vij = pi qj − qi pj = aik pk ajl ql − ain qn ajm pm = aik ajl (pk ql − qk pl ) = aik ajl Vkl . This shows that Vij is a second-rank tensor. Furthermore, it is antisymmetric since Vij = −Vji . Hence: The components of a cross product (an axial vector or an axial tensor 2 of rank 1) are the components of the polar second-rank antisymmetric tensor [V ] deﬁned above.

The axial vector W with components wk and the antisymmetric tensor [V ] deduce from each other through relations: 1 and Vij = δijk wk (10.17) wk = δkij Vij 2 as can be checked easily. 1. We will show in Appendix 18A that this symbol is a rank-3 axial tensor, also called the permutation tensor. 2. The general deﬁnition of an axial tensor is given in Appendix 18A.

222

Symmetry and Physical Properties of Crystals

10.7. Exercises Exercise 10.1 Consider a monoclinic crystal with point group 2, where the basis vector b of the unit cell is perpendicular to the vectors a and c, and a rank-2 symmetric tensor [T ] representing a physical property of this crystal. The components Tij of this tensor, in an orthonormal axis system (Ox1 x2 x3 ) where axis Ox2 is parallel to b, are T11 = 1, T22 = 2, T33 = 3, T13 = T31 = 4 and the other components are zero. 1.

Calculate the components Tij of this tensor in an axis system (Ox1 x2 x3 ) deduced from (Ox1 x2 x3 ) through a rotation by π around Ox3 .

2.

Calculate the components Tij of the same tensor in an axis system (Ox1 x2 x3 ) deduced from (Ox1 x2 x3 ) through a rotation by π around axis Ox2 .

Exercise 10.2 Consider a monoclinic crystal. Its electrical conductivity [σ] is represented in an orthonormal axis system (Ox1 x2 x3 ), where axis Ox2 is parallel to the 2-fold axis, by the following matrix: √ ⎞ ⎛ 7 0 3 ⎝ 0 8 0 ⎠ √ 3 0 5 where the unit is 107 Ω−1 m−1 . 1.

This crystal is submitted to an electric ﬁeld E. Determine the current density vector for the following cases: (a) E is parallel to axis Ox1 , (b) E is parallel to axis Ox2 , (c) E is parallel to axis Ox3 , (d) E is parallel to the bisector of the angle between axes Ox3 and Ox1 , (e) E is in the plane (Ox3 , Ox1 ), and its direction deduces from that of Ox3 through a rotation by 60◦ around Ox2 . What is your conclusion?

2.

A plate with faces parallel to the plane (Ox1 x2 ) is cut out of this crystal, and submitted to an electric ﬁeld E parallel to axis Ox3 . (a) Calculate the component jn of j along the applied ﬁeld (b) What is the meaning of the ratio jn /E, where E is the norm of E?

3.

Express tensor [σ] in a new system of axes, rotated by 60◦ around Ox2 with respect to the preceding one. What do you conclude?

Chapter 10 – Second-rank tensors

223

Exercise 10.3 Let σij be the electrical conductivity tensor of a crystal exhibiting a 3-fold axis. We choose an orthonormal axis system (Ox1 x2 x3 ) such that axis Ox3 is parallel to this axis. 1.

Give the form of this tensor in this axis system.

2.

Calculate the conductivity σs in a general direction, parallel to the unit vector s with direction cosines (s1 , s2 , s3 ). Express it as a function of the non-zero components σij and of the spherical coordinates (r = 1, θ, ϕ) of s. What do you conclude?

Exercise 10.4 1.

Using the direct inspection method, determine the form of a symmetric rank-2 tensor representing a physical property of a crystal with point group ¯4 when it is described in an orthonormal axis system (Ox1 x2 x3 ) in which axis Ox3 is parallel to the ¯4-fold axis and origin O is at the center of symmetry associated with the rotoinversion by π/2.

2.

Now consider a crystal with point group ¯42m, and choose axis Ox1 perpendicular to the mirror. Show that adding this symmetry element does not change the form of the tensor.

Chapter 11

The stress tensor The elastic properties of materials relate the applied stress tensor to the resulting strain tensor via the stiﬀness tensor or its inverse, the compliance tensor. They are the topics of Chapters 11, 12 and 13. In the present chapter, the stress tensor at a point in the material is deﬁned. The basic relations which must be veriﬁed by its spatial derivatives are then determined, and they lead to the condition that this tensor must be symmetric.

11.1. Introduction In Chapters 11, 12 and 13, we investigate the mechanical properties of crystals, i.e. the way they deform under external forces. These external forces induce stresses at each point in the crystal. The relation between the stresses in a material and the external forces applied to its surface is investigated in treatises on the mechanics of continuous media (see for example [1, 2]). Here, we use a few results of mechanics, in particular to locally deﬁne the stress tensor (Chap. 11) and the strain tensor (Chap. 12). At any given point in the crystal, these tensors are related to each other by a material tensor: the compliance tensor, connecting the stress to the strain, or the stiﬀness tensor, connecting conversely the strain to the stress.

11.2. Stress tensor 11.2.1. Introduction In an undeformed solid at equilibrium, each atom or molecule is in an equilibrium position which results from the equality of the attractive and repulsive forces exerted on each of them by the neighboring atoms or molecules (Chap. 8). If the solid is submitted to external forces, it deforms. The external forces are transmitted from atom to atom. Each atom (or molecule) is thus submitted to an additional force, which displaces it to a position where, in the new

© Springer Science+Business Media Dordrecht 2014 C. Malgrange et al., Symmetry and Physical Properties of Crystals, DOI 10.1007/978-94-017-8993-6_11

225

226

Symmetry and Physical Properties of Crystals

equilibrium state, this force is balanced by a restoring force which tends to return the atom or molecule to its initial position. The solid is said to be submitted to stress. Since we are interested in macroscopic properties of the solid, we do not consider an atom but a small volume Δv of the solid, bounded by its surface S (Fig. 11.1). The stresses then lead to forces which the surrounding solid exerts on volume Δv through all elements dS of surface S. More precisely, the solid around Δv exerts on each element dS a force which is proportional to the value of dS: dF = T(r, n)dS. r is the radius vector to the center P of dS : r = O P, and n a unit vector perpendicular to dS, oriented from within Δv to the outside. T(r, n) is a force per unit surface, called the stress at point r; it normally depends not only on r but also on the orientation, deﬁned by n, of the surface on which it acts.

n P dS v S r O’ V

Figure 11.1: Schematic diagram illustrating the surface forces acting on a volume element Δv For a given elementary surface dS, we can consider the material on one side or the other side of the surface. If the normal is oriented from part 1 toward part 2, i.e. if it corresponds to n1 on Figure 11.2, then T(r, n1 )dS represents the force dF2/1 exerted by part 2 on part 1 of the solid. Conversely, for the opposite normal n2 = −n1 , we have T(r, n2 )dS = dF1/2 , which represents the force exerted by part 1 on part 2. The action-reaction law (Newton’s third law) requires these two forces to be equal and opposite: dF1/2 = −dF2/1 We set n1 = n and

and

T(r, n2 )dS = −T(r, n1 )dS.

T(r, n) = −T(r, −n).

The force per unit area T(r, n) is designated as the stress exerted across the small surface element dS, centered at point P such that O P = r, with normal unit vector n, by the part of the solid located on the side toward which vector n is pointing onto the other part. To make the notations simpler, T(r, n) is

Chapter 11 – The stress tensor

227

n1

dF½

dS

dS

dF²⁄1

n2

Figure 11.2: Forces acting on a surface element dS of a solid written as Tn , and it is enough to designate the point P at the center of the small surface element. The volume element Δv can also be submitted to forces proportional to its volume, which will be generally noted fΔv. The simplest example of such a bulk force is the gravity force, equal to ρgΔv where ρ is the mass per unit volume of the solid and g the acceleration of gravity.

11.2.2. Deﬁnition of the stress tensor Consider again the small plane surface element dS centered at P, and its normal vector n. Choose an orthonormal system of axes (Ox1 x2 x3 ) whose origin is located at point O very near dS, and on the side opposite to n (Fig. 11.3). Surface dS intersects axes Ox1 , Ox2 and Ox3 at A, B and C respectively. We thus deﬁne a small tetrahedron, formed by surface ABC and three faces OBC, OCA and OAB respectively perpendicular to Ox1 , Ox2 and Ox3 (Fig. 11.3). x3 TnS(ABC)

C

–T1S(OBC) n

– T2S(OAC) O A

B

x2

– T3S(OAB)

x1

Figure 11.3: Forces acting on the tetrahedron OABC This tetrahedron, with volume Δv, is submitted, through its four faces, to forces related to the stresses deﬁned above, exerted upon it by the part of the solid which is outside. It can also be submitted to bulk forces f Δv. Since this tetrahedron is at equilibrium, the resultant of these forces is zero. The force acting on surface ABC is Tn S(ABC) , in accordance with the deﬁnition of Tn given above.

228

Symmetry and Physical Properties of Crystals

The forces acting on the other faces of the tetrahedron are: on OBC: – T1 S(OBC) , on OCA: – T2 S(OCA) , on OAB: – T3 S(OAB) . Here, we call by convention Ti the stress acting on a surface normal to axis Oxi , with its normal oriented toward the positive Oxi (in other words, the stress exerted by the solid lying on the positive xi side onto the solid lying on the negative xi side). In the case of the forces applied by the surrounding medium upon tetrahedron OABC, the normals to the surfaces OBC, OAC and OAB are oriented respectively toward the negative Ox1 , Ox2 , Ox3 . This explains the minus signs. The equilibrium condition for the tetrahedron is given by: −T1 S(OBC) − T2 S(OCA) − T3 S(OAB) + Tn S(ABC) + f Δv = 0.

(11.1)

We now express the areas of triangles OAB, OBC and OCA as a function of the area of triangle ABC. We note that OAB is the projection of area ABC onto plane (Ox1 ,Ox2 ), which is normal to Ox3 , hence S(OAB) = S(ABC) cos(n, Ox3 ) = n3 S(ABC) where we note n1 , n2 , n3 the direction cosines of vector n. In the same way: S(OBC) = S(ABC) cos(n, Ox1 ) = n1 S(ABC) , S(OCA) = S(ABC) cos(n, Ox2 ) = n2 S(ABC) . We can thus write relation (11.1) in the form: Tn S(ABC) − T1 n1 S(ABC) − T2 n2 S(ABC) − T3 n3 S(ABC) + f Δv = 0. Allowing volume Δv to tend to zero, the ratio Δv/S(ABC) tends to zero, and we can write: Tn = n 1 T1 + n 2 T2 + n 3 T3 . Projecting this equation onto the three axes, we obtain (Tn )1 = T11 n1 + T12 n2 + T13 n3 (Tn )2 = T21 n1 + T22 n2 + T23 n3 (Tn )3 = T31 n1 + T32 n2 + T33 n3 where we denote by Tij the component parallel to Oxi of the stress Tj . The three above equations can be written in the following condensed form: (Tn )i = Tij nj

(11.2)

where (Tn )i is the component parallel to Oxi of the stress exerted on the face ABC normal to the unit vector n, with components nj , by the part of the

Chapter 11 – The stress tensor

229

material located on the side toward which n points onto the part located on the other side of ABC. This relation shows that the coeﬃcients Tij relate vector n, normal to face ABC, to the vector Tn representing the stress acting on this face. We saw (Sect. 9.4.2) that, if two vector quantities A and B, with components respectively Ai and Bi , are related by Bi = Tij Aj , then the Tij are the components of a second-rank tensor [T ]. Hence we can write: Tn = [T ]n. The stress tensor [T ] describes an external action which depends, not on the crystal itself, but on the forces which are applied on its surface by the external world. It is a ﬁeld tensor. The component Tij of this tensor is the component parallel to axis Oxi of the force per unit area (the stress) exerted on a surface element normal to Oxj by the part on the positive Oxj side of the solid onto the part located on the negative xj side. Tij component

face

We have deﬁned the tensor Tij at point P as Tij (r). In the special case where Tij does not depend on the position of P in the solid, the stress tensor is said to be uniform.

11.2.3. Normal stress and shear stress The diagonal terms of the stress tensor [T ] represent stresses which are called normal because they are the forces perpendicular to the surfaces. For example, T11 is the component parallel to axis Ox1 of the force acting on a surface normal to Ox1 . A positive value of T11 represents a tensile stress whereas a negative value represents a compressive stress. The non-diagonal terms Tij (with i = j) represent the shear components on these faces. For the same stress tensor, we now express the normal stress Tν and shear stress τ for a general surface dS, with normal n, a unit vector with components n1 , n2 , n3 (Fig. 11.4). The components (Tn )i of the stress force Tn applied to the surface dS are given by relation (11.2), viz. (Tn )i = Tij nj . The normal stress Tν = Tν n is the projection of Tn on n and Tν = n · Tn = ni (Tn )i , Tν = ni nj Tij

230

Symmetry and Physical Properties of Crystals T Tn

dS

n

Figure 11.4: Normal stress Tν and shear stress τ acting on a surface dS, with normal n, submitted to stress Tn which can be written in matrix form: ⎛ Tν = n1 n2 n3 ⎝ Tij

⎞⎛

⎞ n1 ⎠ ⎝ n2 ⎠ . n3

Using result (10.7), we deduce that the normal stress Tν is equal to the reciprocal of the square of the length of the radius vector of the quadric representing the stress tensor. The shear stress τ is the projection of Tn on the surface element dS: τ = Tn − Tν n which can also be written as

τ = n × (Tn × n)

since n × (Tn × n) = (n · n)Tn − (n · Tn )n = Tn − Tν n.

11.3. Basic relation In many cases, the stress tensor is not uniform. It varies from point to point in the solid and is noted Tij (r). We now calculate the resultant of the forces to which a small parallelepiped, with sides parallel to Ox1 , Ox2 and Ox3 respectively equal to Δx1 , Δx2 , Δx3 , is submitted, taking into account the possibility of bulk forces f per unit volume. We start by calculating the algebraic sum of the components of the stress forces parallel to Ox1 , T1i dS (Fig. 11.5). The components acting on the faces perpendicular to Ox1 give: [T11 (x1 + Δx1 ) − T11 (x1 )]Δx2 Δx3 =

∂T11 Δx1 Δx2 Δx3 . ∂x1

Those acting on the faces perpendicular to Ox2 give: [T12 (x2 + Δx2 ) − T12 (x2 )]Δx1 Δx3 =

∂T12 Δx2 Δx1 Δx3 ∂x2

Chapter 11 – The stress tensor

231

x3 T13(x3 +x3)x1x2 –T11(x1)x2x3 x3

–T12(x2 )x1x3 T11(x1+x1)x2x3

T12(x2 +x2)x1x3 x2

–T13(x3)x1x2 x1

x1

x2

Figure 11.5: Components parallel to axis Ox 1 of the non-uniform stress forces acting on the faces of a rectangle parallelepiped with sides Δx 1 , Δx 2 and Δx 3 and those acting on the faces perpendicular to Ox3 give: [T13 (x3 + Δx3 ) − T13 (x3 )]Δx1 Δx2 =

∂T13 Δx3 Δx1 Δx2 ∂x3

hence, in total: ∂T1j Δx1 Δx2 Δx3 . ∂xj The component parallel to Ox1 of the resultant of the bulk forces is f1 Δx1 Δx2 Δx3 . Let F be the ﬁnal resultant of the stress forces and of the bulk forces acting on unit volume of the material. Its component parallel to Ox1 , F1 , is: F1 =

∂T1j + f1 . ∂xj

The same argument applied to the two other components of F makes it possible to ﬁnally write: Fi =

∂Tij + fi . ∂xj

(11.3)

Since the solid is at equilibrium, Fi = 0, and we obtain: ∂Tij + fi = 0. ∂xj

(11.4)

If the bulk forces are negligible with respect to the stresses: ∂Tij = 0. ∂xj

(11.5)

232

Symmetry and Physical Properties of Crystals

Relation (11.3) will be used in Chapter 14 to investigate the propagation of matter displacements (elastic waves). Since the solid is then no more at equilibrium, it will be applied to Newton’s second law. Relation (11.4) can also be derived in a more formal way by writing the equilibrium condition for a volume V of the solid, submitted to bulk forces f per unit volume and to surface forces FS per unit area, represented by tensor [T ]: f dV + dFS = 0, V

or

S

f (r)dV + V

T(r, n)dS = 0. S

which can be rewritten for each component i, taking relation (11.2) into account: fi (r)dV + Tij (r)nj dS = 0. V

S

Using Ostrogradsky’s theorem,1 we obtain: ∂Tij fi (r)dV + dV = 0 ∂xj V

and

V

fi (r) +

∂Tij dV = 0. ∂xj

V

Since this relation is valid whatever the volume V selected in the solid, we obtain fi +

∂Tij =0 ∂xj

which is the equilibrium relation we were seeking. 1. Ostrogradsky’s theorem states that for a vector ﬁeld A: ∂Aj divAdV = A · ndS or dV = Ak nk dS. ∂xj It can be generalized to the components of a tensor as: ∂Tij Tik nk dS = dV. ∂xj

(11.6)

Chapter 11 – The stress tensor

233

11.4. Symmetry of the stress tensor We now write that, for a solid at equilibrium, the total moment of the forces applied to it is zero. The component Mi of the moment M of a force F (M = r × F) with components Fk is (Sect. 10.6.2) Mi = δijk xj Fk where δijk is the Levi-Civita symbol, or permutation tensor (cf. Appendix 18A.2). Its value is 0 if two subscripts are equal, 1 if the permutation ijk is direct and −1 if it is inverse. The condition on the moment is expressed as: δijk xj fk dV + δijk xj Tkl nl dS = 0. Mi =

(11.7)

The second term can be written, using Ostrogradsky’s theorem:

∂Tkl ∂ (δijk xj Tkl )dV = δijk xj + Tkj dV δijk xj Tkl nl dS = ∂xl ∂xl where we used the fact that: ∂xj = δjl . ∂xl Further, using (11.6): ∂Tkl = −fk . ∂xl We obtain for this second term of (11.7): δijk xj Tkl nl dS = δijk (−xj fk + Tkj )dV and Equation (11.7) becomes: δijk xj fk dV + δijk (−xj fk + Tkj )dV = 0 or

δijk Tkj dV = 0

whatever the volume element dV . Hence δijk Tkj = 0. For i = 1, we obtain T32 − T23 = 0. In the same way, for i = 2 we obtain T13 = T31 and for i = 3 we have T21 = T12 . Thus we showed that Tij = Tji . The stress tensor is symmetric.

234

Symmetry and Physical Properties of Crystals

11.5. Examples of stress tensors In a material, the stress tensor Tij (r) results from the application of surface forces on the external surface Σ of the material, (Tn )Σ . Tij (r) is determined by solving Equations (11.4) with the boundary conditions on surface Σ given by the values of (Tn )Σ at all points of Σ. The solution of this kind of problems is dealt with in treatises on the mechanics of continuous media. In many cases, the solution is a non-uniform stress. It can nevertheless be considered as locally uniform by considering small volume elements, as we will do in the following paragraphs. In experiments designed to measure the elastic properties of materials, the shape of the objects and the applied force conﬁguration are usually designed so that the stress tensor is almost uniform (Sect. 13.1).

11.5.1. Uniaxial stress The stress tensor associated to a uniaxial stress is expressed, in a given frame (Ox1 x2 x3 ), by: ⎛ ⎞ T 0 0 ⎝ 0 0 0 ⎠. 0 0 0 Consider a small cube, with sides parallel to the coordinate axes, and with unit length (Fig. 11.6), and apply relation Tn = [T ]n to its faces. The faces normal to Ox2 and Ox3 are not submitted to any force. Vector n, associated to face ABCD, has the same direction as Ox1 , so that n = i and Tn = T i. If T is positive (as on Fig. 11.6), Tn is a tensile force2 and, if T is negative, Tn is a compressive force. Vector n associated to the opposite face of the cube, OFGH, is equal to −i, and Tn = −T i. We retrieve a tensile force if T is positive, and a compressive force if T is negative. x3 H D

G C

F

O i x1

A

x2

B

Figure 11.6: Uniaxial tensile stress applied on a small cube with unit sides 2. Tn is a force per unit area but here, for simplicity, we assume the surface areas to be equal to unity.

Chapter 11 – The stress tensor

235

11.5.2. Pure shear The stress tensor associated to a pure shear stress is expressed, in a given frame (Ox1 x2 x3 ), as: ⎛ ⎞ 0 T 0 ⎝ T 0 0 ⎠. 0 0 0 Consider, as above, a small cube with sides parallel to the coordinate axes, and with unit length. Figure 11.7 shows the forces acting on it if T is positive. x3

O

x2

x1

Figure 11.7: Pure shear stress acting on a small cube with unit sides If we rotate the coordinate system by 45◦ around Ox3 , the tensor, when expressed in this new set of axes, takes the form (Exercise 11.3): ⎛ ⎞ T 0 0 ⎝ 0 −T 0 ⎠ . 0 0 0 This is a bi-axial stress acting on the surfaces enclosing an angle of 45◦ wih the surfaces perpendicular to Ox1 and Ox2 (Fig. 11.8b).

11.5.3. Hydrostatic pressure Regardless of the orientation of the surface on which it acts, hydrostatic stress is normal to the surface and has the same value p. This stress is represented by tensor: ⎛ ⎞ −p 0 0 ⎝ 0 −p 0 ⎠ 0 0 −p which can be written as: Tij = −pδij , where δij is the Kronecker symbol. In this case, the three components dFi of the force dF acting on a surface element

236

Symmetry and Physical Properties of Crystals x2

x2 x’2

x’1

x1

x1

(a)

(b)

Figure 11.8: (a) Pure shear stress acting on the faces of a small cube with unit sides. (b) This stress is equivalent to a bi-axial stress involving tensile and compressive components, with the same norm, acting on faces at 45◦ to the initial ones. dS perpendicular to unit vector n, with direction cosines ni , are (Eq. 11.2): dFi = Tij nj dS = −p δij nj dS = −p ni dS and

dF = −p ndS

which means a force parallel to n and with value p dS whatever the orientation of n. The minus sign indicates that the pressure force points toward the inside of the volume element (compressive force).

11.6. Eﬀect of gravity Consider a bar in the shape of a rectangle parallelepiped with square crosssection and height h, resting in equilibrium on a plane surface (Fig. 11.9). This bar is submitted to no external stress on any of its faces, except for the one which rests on the surface (stress from the supporting surface). We choose a coordinate system (Ox1 x2 x3 ) parallel to the sides of the parallelepiped, with the axis Ox3 vertical and pointing downward, and the origin O in the plane of the upper face of the bar. The system of Equations (11.4) takes the form: ∂T1j =0 ∂xj ∂T2j =0 ∂xj ∂T3j + ρg = 0 ∂xj

(11.8a) (11.8b) (11.8c)

where ρ is the mass per unit volume of the material and g the acceleration of gravity.

Chapter 11 – The stress tensor

237 O

x1

x2

h

x3

Figure 11.9: Bar in the shape of a rectangle parallelepiped with square cross-section, with height h, resting in equilibrium on a plane surface The faces perpendicular to Ox1 and Ox2 are submitted to no stress, so that Tj2 = Tj1 = 0 on the faces. In a ﬁrst approximation, we may therefore consider that, in a cross section of the bar at x3 = const, the stress is uniform, so that Tj2 = Tj1 = 0 and Tj3 = const over the whole surface. We deduce that:

∂Tj2 ∂Tj2 ∂Tj1 ∂Tj1 = = = =0 ∂x2 ∂x1 ∂x1 ∂x2

and in particular ∂T32 ∂T31 = = 0. ∂x2 ∂x1 Equation (11.8c) then reduces to: ∂T33 + ρg = 0. ∂x3 The solution of this equation is: T33 = −ρgx3 + C(x3 ). C is a constant which depends neither on x1 nor on x2 since the stress is supposed to be uniform at constant x3 . Face x3 = 0 is submitted to no stress, hence T33 (x3 = 0) = 0. We deduce that C(x3 ) = 0 and that T33 = −ρgx3 . On the lower face of the bar (x3 = h), T33 = −ρgh. The force acting on this face of the bar, with area S, is then equal to −ρghS, i.e. to −P if P is the weight of the bar. The surface on which it rests exerts upon the bar a force equal and opposite to its weight, as expected.

238

Symmetry and Physical Properties of Crystals

In metallurgy, test specimens have height around 100 mm. The stress due to gravity therefore varies from zero to the maximum value ρgh which, in the case of a steel specimen for example (ρ = 7.8 kg dm−3 ) is equal to (7.8 × 103 ) × 9.81 × 0.1 = 7.7 × 103 Pa. This stress is therefore completely negligible with respect to the stresses, of the order of a MPa, applied to the specimens in the elastic range. Gravity can thus be neglected.

11.7. Exercises Exercise 11.1 Consider a uniaxial stress T acting on a surface perpendicular to the vector n, with direction cosines n1 , n2 , n3 in an orthonormal axis system (Ox1 x2 x3 ). Determine the components of the stress tensor in the axis system (Ox1 x2 x3 ). First express the tensor in a system of axes where one of the axes, say Ox1 , is parallel to n, and then perform the axis change. Exercise 11.2 Consider a stress tensor which, in a given orthonormal axis system (Ox1 x2 x3 ), takes the form: ⎛ ⎞ 0 0 0 ⎝ 0 0 0 ⎠. 0 0 T 1.

Calculate the moduli Tν and τ of the normal and shear stresses respectively, to which a surface perpendicular to the unit vector n with direction cosines n1 , n2 , n3 is submitted.

2.

For what directions of vector n is the shear stress maximum?

Exercise 11.3 Consider a pure shear tensor represented in an orthonormal axis system (Ox1 x2 x3 ) by: ⎛ ⎞ 0 T 0 ⎝ T 0 0 ⎠. 0 0 0 Give the form of this tensor in an axis system deduced from (Ox1 x2 x3 ) by a 45◦ rotation around Ox3 . Exercise 11.4 The stress tensor [T ] at a point M in a material is given, in an orthonormal axis system (Ox1 x2 x3 ), by: ⎛ ⎞ 0.7 3.6 0 ⎝ 3.6 2.8 0 ⎠ 107 N m−2 . 0 0 7.6

Chapter 11 – The stress tensor

239

1.

Determine the principal stresses and their directions.

2.

Retrieve these results using the Mohr circle method.

3.

Calculate the stress T acting √ on a small surface, centered at M, whose normal has direction cosines ( 3/2, 1/2, 0). Find the normal stress and shear stress components.

240

Symmetry and Physical Properties of Crystals

References [1] D. Calecki, Physique des milieux continus, vol. 1, Mécanique et thermodynamique (Hermann, Paris, 2007) [2] L.D. Landau and E.M. Lifshitz, Course of Theoretical Physics, vol. 7, Theory of Elasticity, 3rd edn. (Elsevier, Oxford, 1986)

Chapter 12

Deformation of a solid. The strain tensor This chapter introduces the displacement gradient tensor, or distortion tensor, which describes the most general distortion of a crystal. This ﬁeld tensor of rank 2 is shown to decompose into the strain tensor, which is symmetric, and an antisymmetric tensor associated to a rotation. The last section is devoted to the thermal expansion of crystals.

12.1. Distortion tensor (displacement gradient tensor) 12.1.1. Deﬁnition We consider a material submitted to a deformation. This deformation displaces point P, deﬁned by its position vector OP = r, to point P such that PP = u(r) (Fig. 12.1). Vector u(r) is the displacement vector at point P. It is not uniform, because if it were, the whole material would simply be translated and it would not be deformed. A neighboring point Q such that PQ = Δr displaces to Q such that QQ = u(r + Δr). x3

Q’

r’ P’

u(r + r)

u(r) P

r

Q

O

x2

x1

Figure 12.1: Transformation of vector PQ= Δr into vector P Q = Δr after deformation

© Springer Science+Business Media Dordrecht 2014 C. Malgrange et al., Symmetry and Physical Properties of Crystals, DOI 10.1007/978-94-017-8993-6_12

241

242

Symmetry and Physical Properties of Crystals

Vector PQ becomes, after transformation, vector P Q = Δr such that: P Q = P P + PQ + QQ Δr = Δr + u(r + Δr) − u(r)

so that

Δr = Δr + Δu

or

(12.1)

if we note Δu = u(r + Δr) − u(r). We can replace u(r + Δr) by its expansion to ﬁrst order, and thus obtain for the three components of Δu: Δui =

∂ui Δxj . ∂xj

(12.2)

∂ui = eij , ∂xj

Setting

Δui = eij Δxj .

we obtain:

(12.3)

Coeﬃcients eij connect the components of a vector Δr to the components of vector Δu. They are therefore the components of a tensor (see Sect. 9.4.2) called the displacement gradient tensor, or distortion tensor, and we can write: Δu = [e]Δr. Thus

Δr = Δr + [e]Δr = ([E] + [e])Δr

or

Δxi

(12.4) (12.5)

= Δxi + eij Δxj = (δij + eij )Δxj

where [E] is the unit tensor. If components eij do not depend on the position of the point, the distortion is uniform, and there are no additional terms in the expansion (12.2). Relations (12.4) and (12.5) are then valid even if points P and Q are not near each other, and the linear relation between Δr and Δr shows that a line remains a line and a plane remains a plane after distortion. If the eij vary from point to point, the distortion is no more uniform, but Equations (12.4) and (12.5) remain valid locally, which implies small Δr. We can thus consider, as is done in this chapter, that the distortions are uniform: if they are not, the properties obtained are valid locally. Further, we will only consider, in what follows, very small displacement gradients (distortions), i.e. eij 1.

Chapter 12 – Deformation of a solid. The strain tensor

243

12.1.2. Physical meaning of components eij We will simplify the interpretation of components eij by considering a twodimensional system, in which we choose an orthonormal axis system (Ox1 x2 ). Equations (12.3) now become the following detailed equations: Δu1 = e11 Δx1 + e12 Δx2 ,

(12.6)

Δu2 = e21 Δx1 + e22 Δx2 .

(12.7)

Consider a rectangle whose sides PQ and PS, respectively parallel to Ox1 and Ox2 , have components (Δx1 , 0) and (0, Δx2 ) respectively. Vectors PQ and PS become, after deformation, P Q and P S respectively. Consider for a start vector PQ, which turned into P Q , and apply relations (12.6) and (12.7): Δu1 = e11 Δx1 , Δu2 = e21 Δx1 . PQ has rotated by angle θ, and its length has changed. As we immediately see on Figure 12.2, tan θ = Δu2 /(Δx1 + Δu1 ). Since we assume that eij 1, Δu1 and Δu2 are much smaller than Δx1 and tan θ ∼ = Δu2 /Δx1 = e21 , and tan θ ∼ θ. We can write: = θ = e21 . Thus e21 is the angle by which PQ, parallel to Ox1 , has rotated. It is counted as positive in the sense from Ox1 to Ox2 (direct sense). The same argument applied to PS shows that e12 is the angle θ by which PS, parallel to Ox2 , has turned, counting it as positive from Ox2 to Ox1 (clockwise).1 x2

R’ S’ ’

S

R P’

x2

x1

u1

Q

P O

Q’ u2

x1

x1

Figure 12.2: Distortion of rectangle PQRS, which becomes P Q R S . The lengths Δu 1 and Δu 2 are hugely magniﬁed in order to make angle θ visible.

1. It is obvious that, to keep Figure 11.2 and the following ones clear, it is necessary to show lengths Δu1 and Δu2 much larger than in reality. Therefore, they do not satisfy the condition eij 1, and angles θ and θ are also too large.

244

Symmetry and Physical Properties of Crystals

We now calculate the variation in length Δx1 of PQ, which became P Q : we have P Q − PQ = P Q − Δx1 . We see on Figure 12.2 that Δx1 + Δu1 = P Q cos θ ∼ = P Q since θ 1. Thus P Q ∼ = PQ + Δu1 , and we obtain Δu1 P Q − PQ = e11 . = PQ Δx1 The relative elongation of PQ is thus equal to e11 . The same argument applied to PS shows that e22 is the relative elongation of PS, parallel to Ox2 . These results are easily generalized to three dimensions. We can thus state that: each diagonal term2 eii in the distortion tensor represents the relative elongation of a segment parallel to axis Oxi , the components eij , where i = j, describe the rotation of these segments.

12.2. Decomposition of the distortion tensor into a rotation and a strain 12.2.1. Introduction using a simple example Consider the very simple distortion tensor ⎛ 0 −α ⎝α 0 0 0

[T ] represented by matrix ⎞ 0 0⎠ . 0

This distortion does not aﬀect a vector parallel to Ox3 , and we can therefore focus on the distortion in plane (Ox1 ,Ox2 ) and investigate what a small square PQRS becomes after distortion (Fig. 12.3). The diagonal terms being zero, the segments parallel to Ox1 and Ox2 retain their lengths. Segment PQ undergoes a rotation by α in the direct sense and segment PS a rotation −α in the clockwise direction, i.e. a rotation by α in the direct sense. Thus the square has been transformed into an identical square, rotated by angle α in the direct sense. This shows that there are distortions which do not deform the solid, but just rotate it.

2. Here, Einstein’s convention does not apply to notation eii , i.e. no sum is implied.

Chapter 12 – Deformation of a solid. The strain tensor

245

R’ x2

S’

S

R

Q’

P’

P

Q

O

x1

Figure 12.3: Transformation of square PQRS when submitted to a special distortion involving a simple rotation

12.2.2. Expressing the distortion associated to small rotations Consider a small rotation by angle dα around an axis with unit vector n going through point O. Let M be the transform of point M in this rotation (Fig. 12.4). OM = OM + MM . The plane perpendicular to the rotation axis, going through M, intersects this axis at H.

H

d

M’ M

n O

Figure 12.4: Transformation of vector OM into vector OM through a small rotation, by angle d α, around an axis with unit vector n going through point O Since we assume angle dα to be very small, arc MM and its tangent at M are very close to each other. MM is perpendicular to n and also to HM since the rotation angle dα is small. MM , being perpendicular to plane (OH, HM), is thus perpendicular to OM and to n, hence parallel to vector n × OM. Its length MM is MM = HM dα = OM sin θ dα

246

Symmetry and Physical Properties of Crystals

where θ is the angle between OM and n. We thus obtain MM = (n × OM) dα OM = OM + (n × OM) dα.

and

(12.8)

If we denote as ni the components of n and xi the components of OM in any given orthonormal axis system (Ox1 x2 x3 ), the vector n × OM has for components, in this axis system ⎧ ⎨ n 2 x3 − n 3 x2 n x − n 1 x3 ⎩ 3 1 n 1 x2 − n 2 x1 and Equation (12.8) can be written as OM = ([E] + [Ω])OM where [Ω] is a tensor (since it relates vector OM − OM to vector OM) which, in the orthonormal basis chosen, is expressed as ⎞ ⎛ n2 0 −n3 0 −n1 ⎠ [Ω] = ⎝ n3 −n2 n1 0 and [E] is the unit tensor. We deduce that any vector r transforms, under rotation by a small angle dα around n, into vector r such that r = ([E] + [Ω])r

(12.9)

where [Ω] is an antisymmetric tensor. We note that the special case we discussed in Section 12.2.1 satisﬁes this result. Since this relation is linear, it applies to any vector Δr, irrespective of whether its origin is on the rotation axis. Relation (12.9) then becomes: Δr = ([E] + [Ω])Δr or

Δu = Δr − Δr = [Ω]Δr.

[Ω], an antisymmetric tensor, is associated to the rotation vector ndα. We thus ﬁnd a second example of an axial vector, the rotation vector ndα being equivalent to the antisymmetric second-rank tensor [Ω]dα (see Sect. 10.6.2).

12.2.3. Strain tensor A general distortion tensor can be decomposed into the sum of a symmetric tensor [S] and an antisymmetric tensor [A] (Sect. 10.1.1), which we will denote here as [Ω], such that: Sij =

eij + eji 2

Ωij =

eij − eji , 2

Chapter 12 – Deformation of a solid. The strain tensor so that

∂uj 1 ∂ui + 2 ∂xj ∂xi

∂uj 1 ∂ui . − Ωij = 2 ∂xj ∂xi Sij =

247

(12.10) (12.11)

Relation (12.5) becomes Δr = ([E] + [e])Δr = ([E] + [S] + [Ω])Δr. The distortions we consider here are always small, hence eij 1, and we can write: ([E] + [S] + [Ω]) ∼ = ([E] + [S])([E] + [Ω]), and

Δr = ([E] + [S])([E] + [Ω])Δr.

The transformation of vector Δr into Δr is the product of a rotation ([E]+[Ω]) and a deformation ([E] + [S]).3 [S] is the symmetric part of the distortion tensor: it is called the strain tensor. [Ω], its antisymmetric part, is called the rotation tensor. Generally, interest focuses only on the change in shape of the object, hence on the strain tensor [S], a symmetric tensor. The diagonal terms in [S] are equal to those of [e], and they thus represent relative elongations (see Sect. 12.1.2). Thus S11 represents the relative elongation of a segment parallel to axis Ox1 , S22 that of a segment parallel to Ox2 and S33 that of a segment parallel to Ox3 . The strain tensor is a ﬁeld tensor. It usually results from another ﬁeld tensor being applied to the crystal, for example a stress, deﬁned in Chapter 11, an electric ﬁeld if the crystal is piezoelectric (Chap. 15), or a variation in temperature as we will see in Section 12.6.

12.3. Elongation in a given direction There is often interest in the relative elongation, in a given direction parallel to unit vector s, of a material submitted, in the vicinity of point P, to a given strain tensor [S]. If [S] is uniform, Δ/|s represents the relative elongation of a bar parallel to s. The tensor is given through its components Sij in a given orthonormal axis system (Ox1 x2 x3 ). Let (Ox1 x2 x3 ) be a new orthonormal axis system such that Ox1 is parallel to s. We saw in last section that the relative elongation in direction Ox1 is given by S11 . Thus Δ = S11 = a1i a1j Sij , s 3. The order of the operations is irrelevant: since Ωij 1 and Sij 1, ([E] + [S])([E] + [Ω]) ∼ = ([E] + [Ω])([E] + [S]).

248

Symmetry and Physical Properties of Crystals

where {aij } is the transformation matrix leading from axis system (Ox1 x2 x3 ) to axis system (Ox1 x2 x3 ). The basis vector e1 of the new system is none other than s, hence a1i = si . We obtain Δ = si sj Sij (12.12) s or, in matrix form, ⎛ Δ = s1 s2 s3 ⎝ s

⎞⎛ Sij

⎞ s1 ⎠ ⎝ s2 ⎠ . s3

This relative elongation is equal to the reciprocal of the square of the radius vector of the quadric associated to tensor [S] (Sect. 10.3.2).

12.4. Volume expansion (volumetric strain) When described in the axis system (Ox1 x2 x3 ) of its principal axes, a strain tensor [S], with components Sij , is diagonal. Consider a small rectangle parallelepiped with sides parallel to Ox1 , Ox2 and Ox3 and with lengths respectively Δx1 , Δx2 , Δx3 (Fig. 12.5). x3 x2(1+S22) x1(1+S11) x1 O

x2

x3

x3(1+S33) x2

x1

Figure 12.5: A rectangle parallelepiped with sides parallel to principal axes Ox 1 , Ox 2 and Ox 3 , with lengths respectively Δx 1 , Δx 2 , Δx 3 , shown before and after deformation This rectangle parallelepiped, with volume ΔV equal to Δx1 Δx2 Δx3 , becomes, under this deformation, another rectangle parallelepiped since only the diagonal terms of the tensor are non-zero. Its sides have lengths respectively Δx1 (1 + S11 ), Δx2 (1 + S22 ) and Δx3 (1 + S33 ). The volume ΔV of the deformed parallelepiped is: ΔV = ΔV (1 + S11 )(1 + S22 )(1 + S33 ) ≈ ΔV (1 + S11 + S22 + S33 ).

Chapter 12 – Deformation of a solid. The strain tensor

249

The relative variation in volume is: ΔV − ΔV = S11 + S22 + S33 , ΔV equal to the trace of the matrix representing tensor [S] in the coordinate system of its principal axes. We saw (Sect. 10.1.3) that the trace of a tensor is independent of the coordinate system in which it is expressed. Therefore the relative variation in volume (volume expansion, or volumetric strain) is equal to the trace of the strain tensor whatever the coordinate system in which the tensor is expressed.

12.5. Special cases of strain 12.5.1. Simple elongation The strain tensor associated to simple elongation, expressed in a given axis system (Ox1 x2 x3 ), has a single non-zero term, located on the diagonal; for example: ⎛ ⎞ 0 0 0 ⎝ 0 0 0 ⎠. 0 0 S A small rectangle parallelepiped with sides parallel to the axes and with lengths respectively Δx1 , Δx2 , Δx3 remains a rectangle parallelepiped, in which only the side parallel to Ox3 has suﬀered a relative elongation equal to S.

12.5.2. Pure shear strain The associated strain tensor is expressed, in a given coordinate system (Ox1 x2 x3 ), as: ⎛ ⎞ 0 S 0 ⎝ S 0 0 ⎠. 0 0 0 It is easy to show (Exercise 12.2) that, in the coordinate system (Ox1 x2 x3 ) rotated by 45◦ around axis Ox3 , this tensor takes on the form: ⎛ ⎞ S 0 0 ⎝ 0 −S 0 ⎠ 0 0 0 which corresponds to an expansion along Ox1 and a contraction along Ox2 . A small square PQRT, with sides parallel to Ox1 and Ox2 respectively, becomes after deformation a lozenge (Fig. 12.6). The length of the sides of the lozenge is equal to that of the square since, in the initial coordinate system, S11 = S22 = 0.

250

Symmetry and Physical Properties of Crystals x2

T

R’

T’

R

S

P

S

Q’ Q

O

x1

Figure 12.6: Pure shear of the small square PQRT, with sides parallel to Ox 1 and Ox 2 , which becomes the lozenge PQ R T

12.5.3. Simple shear strain The distortion tensor [e] in simple shear is expressed in a given frame (Ox1 x2 x3 ) as: ⎛ ⎞ 0 γ 0 ⎝ 0 0 0 ⎠. 0 0 0 A small square PQRS with sides parallel to Ox1 and Ox2 becomes, after this distortion, a lozenge PQR S because the tensor has no diagonal terms (Fig. 12.7a). The side parallel to Ox2 rotates by −γ (see Sect. 12.2.1). Because the tensor is not symmetric, we decompose it into a strain and a rotation: ⎛ ⎞ ⎛ ⎞ 0 γ/2 0 0 γ/2 0 [S] = ⎝ γ/2 0 0 ⎠ and [Ω] = ⎝ −γ/2 0 0 ⎠ . 0 0 0 0 0 0 Simple shear thus consists in the combination of a rotation by angle −γ/2 around Ox3 and pure shear (Fig. 12.7b).

12.6. Thermal expansion Suppose we submit a bar of an isotropic material, with length 0 at temperature T0 , to a temperature change ΔT . Its length becomes such that: = 0 (1 + αΔT ) where α is the linear thermal expansion coeﬃcient of the material. In a general way, an isotropic solid submitted to a uniform rise in temperature expands while retaining its shape, and vector Δr in the material becomes, after a change in temperature ΔT , a vector Δr parallel to Δr and such that: Δr = Δr(1 + αΔT ) = Δr + Δu

Chapter 12 – Deformation of a solid. The strain tensor

251

x2 S S’’

R R’’

S S’ S’’ x3

– f

P

R R’’ R’

–– f 2

Q

Q Q’

P

(a)

x1

(b)

Figure 12.7: (a) Simple shear of the small square PQRS, which becomes lozenge PQR S . (b) This transformation can be decomposed into two successive transformations: rotation by −γ/2 (the square PQRS becomes square PQ R S ), and then a deformation of PQ R S analogous to that of Figure 12.6. Δu = αΔT Δr.

with

If the solid is not isotropic, the vector Δu is, in general, no more parallel to Δr and its expression at a function of Δr is given by a strain tensor [S] proportional to the change in temperature ΔT : Δu = [S]Δr = [α]ΔrΔT or and

Δui = αij Δxj ΔT, Sij = αij ΔT.

(12.13)

Tensor [α] thus deﬁned is the thermal expansion tensor. This second-rank tensor is symmetric and represents a physical property of the material. It relates an external applied constraint (the change in temperature) to the eﬀect it induces (strain). It is a material tensor, which must be invariant with respect to the crystal’s symmetry elements. The number of independent coeﬃcients of symmetric rank-2 tensors was determined (Sect. 10.5) for the various point groups. This number depends only on the crystal system because it is found to be identical for all the point groups of a given crystal system. We thus obtain for the various crystal systems the following results: Triclinic system: 6 independent coeﬃcients. Monoclinic system: one principal axis of the tensor is parallel to the 2-fold axis (groups 2 and 2/m) or perpendicular to the mirror (group m). There are four independent coeﬃcients. The ellipsoid representing the tensor has one of its axes parallel to the 2-fold axis or perpendicular to the mirror. Orthorhombic system: the principal axes are parallel to the 2-fold axes or perpendicular to the mirrors. They are the axes of the ellipsoid representing the tensor. There are three independent coeﬃcients.

252

Symmetry and Physical Properties of Crystals

Tetragonal, rhombohedral and hexagonal systems: the ellipsoid representing the tensor is an ellipsoid of revolution around the axis with order larger than 2. There are two independent coeﬃcients. Cubic system: the representation ellipsoid is a sphere. The crystal behaves with respect to thermal expansion as an isotropic material. There is only one coeﬃcient. We note that the strain induced by a change in temperature is uniform if the temperature is uniform. The coeﬃcients αij are in general all positive. Nevertheless there are a few cases where one of the coeﬃcients is negative (calcite or beryl for example). In these special cases, there are directions in which the expansion coeﬃcient is zero. Consider for example calcite, with point group ¯3m, for which the thermal expansion tensor [α] is expressed as: ⎛ ⎞ −5 0 0 ⎝ 0 −5 0 ⎠ 10−6 ◦ C−1 0 0 27 when expressed in an axis system where Ox3 is parallel to the 3-fold axis.4 The relative elongation Δ/|s , in a given direction with unit vector s, is given by Equation (12.12): Δ = si Sij sj = si sj αij ΔT. s If ΔT = 1◦ C, we obtain for calcite: Δ = [−5(s21 + s22 ) + 27s23 ] 10−6 s

which, expressed in spherical coordinates, becomes: Δ = [−5sin2 θ + 27cos2 θ] 10−6 . s The surface representing this relative elongation is obtained by giving any segment parallel to s drawn from a given point O the length Δ/|s . Here it is a surface of revolution around Ox3 . Figure 12.8a shows a section of this surface by a plane going through this axis of revolution. We see that

Δ =0 s

if

tan2 θ =

27 5

thus for all direction at angle θ = θ0 = 66.7◦ (or its supplement θ = 113.3◦ ) to axis Ox3 . 4. We recall that a ¯ 3-fold axis is equivalent to a 3-fold axis and a center of symmetry.

Chapter 12 – Deformation of a solid. The strain tensor x3

253

x3

+ o

_

o

_

+

(a)

(b)

Figure 12.8: Thermal expansion of a crystal of calcite. The 3-fold axis, chosen for the axis Ox 3 , is an axis of revolution and the ﬁgures represent any plane (Oρ, Ox 3 ) going through Ox 3 . (a) Relative elongation for all directions of a plane going through axis Ox 3 . (b) Transformation of a sphere with unit radius, which becomes an ellipsoid of revolution around Ox 3 . The deformations are hugely exaggerated in order to be visible. We saw (Eq. (10.6)) that, for a given tensor with components Tij , the quantity Tij si sj is equal to 1/r 2 where r is the length of the radius vector of the representation quadric for the tensor, deﬁned by Tij si sj = 1. This remark makes it possible to retrieve the above result, viz. the fact that in the directions of the cone asymptotic to the hyperboloids −5(x21 + x22 ) + 27x23 = ±1, the relative elongation is zero since r → ∞. For those directions that enclose with Ox3 an angle smaller than the half-angle of the cone, the representation of the quadric is a two-sheet hyperboloid with equation αij xi xj = 1 and the relative elongation is then equal to 1/r 2 . For directions that are outside this cone, the quadric is a one-sheet hyperboloid with equation αij xi xj = −1 and the elongation is equal to −1/r 2 . Figure 12.8b shows that a sphere with unit radius becomes, through thermal expansion, an ellipsoid with an expansion in the direction Ox3 and a contraction in all directions of plane (Ox1 , Ox2 ). We note that, in direction θ0 , although the radius vector does not expand, it nevertheless undergoes a transformation which is then only a rotation (Exercise 12.5). Any change in temperature of a solid leads to a relative variation ΔV /V of its volume V . As we saw in Section 12.4, ΔV /V is the trace of the strain tensor: ΔV = Sii = αii ΔT = (α11 + α22 + α33 )ΔT V The bulk thermal expansion is αii . If the material is isotropic, with linear expansion coeﬃcient α, we obtain ΔV /V = 3αΔT , as expected.

254

Symmetry and Physical Properties of Crystals

When it is expressed in the coordinate system of its principal axes, tensor [α] is diagonal, and its diagonal terms α11 , α22 , α33 are called the principal expansion coeﬃcients. For simplicity, they are noted α1 , α2 , α3 respectively. A few examples of the numerical values of these coeﬃcients are given in Table 12.1, in units of 10−6 ◦ C−1 . Table 12.1: Principal expansion coeﬃcients for some crystals, in units of 10−6 ◦ C−1 α1

α2

α3

10.8

10.8

64.5

around − 210◦ C

−2

−2

55

Rhombohedral

around 25◦ C

13.4

13.4

7.97

Calcite

Rhombohedral

40◦ C

−5

−5

27

Copper

Cubic

around 25◦ C

16

16

16

Silicon

Cubic

around 25◦ C

2.35

2.35

2.35

Crystal

Crystal system

Zinc

Quartz

Hexagonal

Temperature range 30 to

118◦ C

around

12.7. Exercises Exercise 12.1 A material is distorted in such a way that the components of the displacement u(P) at a point P with coordinates (x1 , x2 , x3 ) in an orthonormal axis system are: u1 = 2 × 10−5 x1 − 10−5 x2 u2 = 2 × 10−5 x1 − 2 × 10−5 x2 u3 = 0 1.

Determine the components eij = ∂ui /∂xj of the distortion tensor [e]. Decompose tensor [e] into the strain tensor and the rotation tensor.

2.

Determine the relative elongation of a segment in a direction parallel to the vector with components (1, 1, 1).

Exercise 12.2 A uniform strain tensor is represented in an orthonormal axis system (Ox1 x2 x3 ) by the matrix: ⎛ ⎞ 0 S 0 ⎝ S 0 0 ⎠. 0 0 0

Chapter 12 – Deformation of a solid. The strain tensor

255

1.

How does this strain transform a square with sides being parallel to Ox1 and Ox2 respectively and with unit length?

2.

Determine the principal values and the principal axes of this tensor.

Exercise 12.3 Consider a homogeneous bar with the shape of an elongated rectangle parallelepiped (see ﬁgure below). Choose an axis system such that Ox1 is parallel to the long side of the bar, Ox2 and Ox3 being parallel to the two other sides. This bar undergoes a uniform strain, the principal axes of which are Ox1 , Ox2 and Ox3 , and the principal values S11 = η, S22 = −0.3η, S33 = −0.3η with η = 10−4 . A line with length L, drawn on the bar in plane (Ox1 , Ox2 ) in the undeformed state, encloses angle α with Ox1 before deformation. x2 L

x1

1.

Calculate the relative elongation of the line.

2.

After deformation, the line encloses with Ox1 the angle α = α + ε. Calculate the small angle ε.

Exercise 12.4 A small distortion of a crystal is deﬁned ⎛ 4 2 eij = ⎝ −4 1 6 0

by the following tensor: ⎞ −2 0 ⎠ 10−6 . 3

Determine the strain tensor Sij and the rotation tensor Ωij . Find the principal axes of tensor [S], the rotation axis and the angle of rotation Δα corresponding to tensor [Ω]. Exercise 12.5 Graphite is hexagonal, with point group 6mm. In order to determine the coeﬃcients of the thermal expansion tensor, the lattice parameters of a graphite crystal were measured at 20◦ C and at 100◦ C. At 20◦ C, the values are: a20 = 2.4560 Å, c20 = 6.6960 Å. At 100◦ C, they are: a100 = 2.4557 Å, c100 = 6.7110 Å.

256

Symmetry and Physical Properties of Crystals

1.

Calculate, in this temperature range, the average thermal expansion tensor5 of graphite. Indicate what axis system it is expressed in.

2.

Calculate the average thermal expansion coeﬃcient in a general direction at angle θ to the 6-fold axis. Show that there are directions in which the elongation is zero, and that these directions form a cone; determine its apical angle θ0 . Give a graphical interpretation of this result using the representation quadric of this tensor.

3.

Show that this special direction undergoes, in a temperature variation, a small rotation; calculate it.

Exercise 12.6 Consider a crystal of rutile TiO2 , with tetragonal symmetry and lattice parameters a = b = 4.5933 Å and c = 2.9592 Å at 0◦ C. When it is heated from 0◦ C to 100◦ C, the angle between planes (100) and (101) decreases by 0.095 mrad. Given that the average bulk expansion between 0◦ C and 100◦ C is 23.4 × 10−6 ◦ C−1 , calculate the two principal expansion coeﬃcients of this crystal. Exercise 12.7 Barium titanate BaTiO3 undergoes several phase changes (or phase transitions) at various temperatures: above 120◦ C, BaTiO3 is cubic. At 120◦ C it becomes tetragonal, and remains so down to 0◦ C. At 0◦ C, BaTiO3 becomes orthorhombic and remains so down to −100◦ C, when it becomes rhombohedral. The point symmetry group and the lattice parameters of the various phases are given in the table below. System P. G. T

Cubic m¯3m

Tetragonal Orthorhombic Rhombohedral 4mm mm2 3m ◦ ◦ ◦ 120 C 0 C − 100 C 120◦ C 120◦ C 0◦ C – 100◦ C a = 4.010 Å a = b = 4.002 Å bm = cm = 4.012 Å a = 3.996 Å c = 4.021 Å am = 3.988 Å α = 89.86◦ ◦ ◦ 0 C α = 90.20 a = b = 3.991 Å – 100◦ C c = 4.034 Å bm = cm = 4.012 Å am = 3.978 Å α = 90.40◦

5. The lattice parameters do not vary linearly with temperature. The data given only allow calculating the average thermal expansion coeﬃcients.

Chapter 12 – Deformation of a solid. The strain tensor

257

In the cubic ↔ tetragonal transformation, the directions of the basis vectors remain unchanged. In the tetragonal ↔ orthorhombic transformation, the direction of a is unchanged. The rectangular face (b, c) becomes a lozenge with side bm = cm = a and with angle α = 90◦ , deﬁning a monoclinic pseudo-unit cell. The orthorhombic unit cell is a unit cell with twice the volume of this one. The basis vector ao is parallel to the vector ac of the cubic unit cell. The vectors bo and co are respectively parallel to the diagonals of the lozenge faces of the monoclinic pseudo-unit cell. The 3-fold axis of the rhombohedral phase coincides with one of the 3-fold axes of the cubic phase. 1.

Calculate the components of the average6 thermal expansion tensor of BaTiO3 in the tetragonal phase. Deduce the expansion coeﬃcient for a general direction. Does it vanish for some directions? Which ones?

2.

Calculate the norms of the basis vectors of the orthorhombic unit cell at 0◦ C and at −100◦ C. Determine the thermal expansion tensor in this phase (express it in the orthonormal axis system parallel to the basis vectors of the orthorhombic unit cell).

3.

Calculate the components of the strain tensor corresponding to the transition from the cubic cell (at 120◦ C) to: (a) the tetragonal unit cell at 120◦ C, (b) the orthorhombic unit cell at 0◦ C, (c) the rhombohedral unit cell at −100◦ C. Indicate, in each case, the axis system in which the tensors are expressed.

6. See the note for Exercise 12.5.

Chapter 13

Elasticity The stiﬀness and compliance tensors, which relate the stress tensor to the resulting strain tensor, are symmetric tensors of rank 4. This chapter shows how the intrinsic symmetry of the strain and stress tensors reduces the number of independent components of the compliance and stiﬀness tensors, and then how the symmetry of the crystal, described by its point group, can further reduce this number. A short notation, called Voigt’s notation, is often used for these tensors. It represents the stress and the strain tensors through 6-component vectors, and the compliance and stiﬀness tensors by symmetric 6 × 6 matrices which are inverse to each other.

13.1. Introduction In this chapter, we investigate the deformation of a crystalline material under the inﬂuence of a given stress. We ﬁrst need to know the stress acting at any point in the material. We saw (Sect. 11.5) that the stress tensor Tij (r) in a material results from the application of surface forces on the external surface Σ of the material. For measurements to have an easy interpretation, the shape of the material and the conﬁguration of the external forces to be applied are designed so that the stress tensor is practically uniform. The most usual experiments consist in measuring the strain resulting from a uniaxial stress. The typical specimen shape for this use is shown on Figure 13.1. 0 S

F

F

5 cm

(a)

(b)

Figure 13.1: (a) Photograph of a tensile test specimen; (b) schematic diagram of a traction experiment. The uniaxial stress T in the central part, with cross section S, is T =F /S.

© Springer Science+Business Media Dordrecht 2014 C. Malgrange et al., Symmetry and Physical Properties of Crystals, DOI 10.1007/978-94-017-8993-6_13

259

260

Symmetry and Physical Properties of Crystals

It consists of a long central cylindrical part with constant cross section, and of two ends with a cross section larger than the central part. The transition between the central part and the ends occurs progressively. The ends of these specimens are secured to the grips. One of them is ﬁxed and the other one submitted to a traction force F. The stress tensor in the central part, with cross section S, can then be shown to be practically uniform. The stress is uniaxial and its value is T = F/S. As a result, the length of the constant cross section part of the specimen increases from the zero-stress value 0 to = 0 + Δ. The elongation Δ depends on the value of the stress. The deformation curves are usually represented by plotting the relative elongation Δ/ horizontally and the stress vertically. The general trend is given on Figure 13.2, where we note that the initial part is a straight line. T Elastic range

Plastic range Fracture

0

Figure 13.2: Deformation curve of a material submitted to a tensile stress. The linear part of this curve is the elastic deformation range. This diagram (T , Δ/) shows several stages in the deformation process: 1. The elastic deformation range For small values of T , the material has a linear behavior. The elongation is proportional to the applied stress: 1 Δ = T. E This is Hooke’s law, and E is Young’s modulus of the material, assumed to be isotropic. In this stress range, the material recovers its initial dimensions when the stress is removed: the transformation is reversible. Young’s modulus is a measure of the mechanical property called stiﬀness or rigidity. The larger Young’s modulus, the more rigid is a material, and therefore the smaller is its elastic deformation for a given value of the stress. Actually, Young’s modulus is not suﬃcient to completely characterize the deformation of the bar, because the cross section of the bar also changes. If the cross section is circular, it remains circular in an isotropic material, and

Chapter 13 – Elasticity

261

its diameter d undergoes a relative contraction, noted Δd/d (with Δd < 0), also proportional to the stress. The absolute value of the ratio between this relative contraction and the relative elongation of the bar is called Poisson’s ratio, noted ν: ν=−

Δd/ d Δ/

so that we can write:

ν Δd = − T. d E We note that, in this range, the volume of the material changes because the elongation is generally not totally compensated by the decrease in cross section. This volume change is noted as: Δ 2Δd 1 − 2ν ΔV = + = T. V d E The order of magnitude of Young’s modulus E for metals is some 1010 N m−2 , and Poisson’s coeﬃcient ν is generally close to 0.3 for usual metals. 2. The plastic range Beyond the elastic range, the strain-stress curve shows a plateau which can be more or less extended depending on the material. This is the plastic deformation range, where deformation occurs at almost constant volume. In this range, which involves the displacement and multiplication of defects called dislocation lines,1 the material retains some permanent deformation when the stress is released. The deformation in this range is thus not reversible. The boundary between the two ranges we just deﬁned is called the elastic limit, or yield strength. It is related to the defects in the solid, and is therefore an extrinsic property of the material, variable from one specimen to another. The order of magnitude of this elastic limit for metals is some 107 to some 108 N m−2 . In practice, this limit is often diﬃcult to pinpoint because the transition from the elastic to the plastic range is continuous. 3. The breaking range In this range, the deformation is localized: the cylinder necks at a point and breaks. This type of diagram assumes that the stress and strain are simultaneous, i.e. that the deformation sets in as soon as the stress is applied. This is the case for metals and many solids. These materials are called elastic materials. Their behavior in a deformation experiment is not inﬂuenced by the stress rate, and 1. A brief introduction to dislocations is given in the complement to this chapter.

262

Symmetry and Physical Properties of Crystals

it is well described by Hooke’s law, independent of time: 1 Δ = T E

or

T =E

Δ .

Some materials, called viscoelastic, feature a time-dependent stress-strain relation. We will not discuss them here. We will therefore restrict discussion to elastic materials and their mechanical behavior in the elastic range.

13.2. Compliance and stiﬀness tensors 13.2.1. Generalized Hooke’s law As we just saw, Young’s modulus is not suﬃcient to characterize the elastic deformation of a bar, since its cross section decreases at the same time as it elongates. Furthermore, we are interested in crystals, and thus in anisotropic materials. We also want to be able to deal with stresses that are not necessarily uniaxial. Hooke’s law must then be generalized. It relates the stress tensor Tij to the strain tensor Sij : Sij = sijkl Tkl .

(13.1a)

Conversely, the stress tensor is related to the strain tensor by relation: Tij = cijkl Skl .

(13.1b)

The coeﬃcients sijkl are called the compliance constants, and the coeﬃcients cijkl the stiﬀness constants.2 Relations (13.1a) and (13.1b) each represents a set of 9 equations which relate the components of a rank-2 tensor ([T ] or [S]) to the components of another rank-2 tensor ([S] or [T ]) through coeﬃcients sijkl or cijkl , which are therefore the components of rank-4 tensors (see Sect. 9.4.2), the compliance tensor [s] for sijkl and the stiﬀness tensor [c] for cijkl . It may be useful to show this in this special case for one of the two tensors, sijkl for example. In a change of orthonormal axis system, Sij becomes Smn and Tkl becomes Tpq such that (Eq. (9.13a) and (9.13b)): = ami anj Sij , Smn Tkl = apk aql Tpq

where {aij } is the transformation matrix from the old to the new axis system. We obtain: = ami anj sijkl Tkl = ami anj sijkl apk aql Tpq Smn

2. The sijkl and cijkl are sometimes called elastic moduli and elastic constants respectively.

Chapter 13 – Elasticity so that

263

= smnpq Tpq Smn

with

smnpq = ami anj apk aql sijkl

(13.2)

i.e. a transformation identical to that of the product of four components. This proves that sijkl is a rank-4 tensor. We can rewrite relations (13.1a) and (13.1b) in the form: [S] = [s][T ], [T ] = [c][S], where [s] is the compliance tensor and [c] the stiﬀness tensor. Since the strain tensor [S] is dimensionless, the components of [s] are dimensionally the inverse of a stress, i.e. m2 N−1 . Typical orders of magnitude for the compliance tensor components are 10−11 m2 N−1 . The stiﬀness tensor components cijkl are expressed in N m−2 and have values on the order of 1011 N m−2 . Example: the central part of the tensile specimen of Figure 13.1 is submitted to a uniform uniaxial stress represented by tensor ⎞ ⎛ T 0 0 ⎝ 0 0 0 ⎠ 0 0 0 in an axis system (Ox1 x2 x3 ) where Ox1 is parallel to the specimen axis. The generalized Hooke’s law (Eq. (13.1a)) provides, for the diagonal components: S11 = s1111 T,

S22 = s2211 T

and

S33 = s3311 T

since only T11 = T is non-zero. These components represent the (algebraic) relative elongations along the specimen axis (S11 ) and perpendicular to it (S22 and S33 ). The two latter components have no reason to be equal, in contrast to the isotropic case. The terms obtained for i = j, Sij = sij11 T , represent shear strains.

13.2.2. Symmetry of the compliance and stiﬀness tensors We saw that the stress tensor is symmetric (Sect. 11.4). We can therefore, in relation (13.1a), collect the terms containing components Tkl and Tlk for which k is diﬀerent from l. The strain Sij thus takes the form: (sijkl + sijlk )Tkl . Sij = sijkk Tkk + kl=23,31,12

Therefore sijkl and sijlk cannot be distinguished, and they are chosen equal: sijkl = sijlk .

264

Symmetry and Physical Properties of Crystals

In the same way, since Sij = Sji (Sect. 12.2.3), we have sijkl = sjikl . Thus sijkl = sijlk = sjikl = sjilk . For the same reasons, we also have: cijkl = cijlk = cjikl = cjilk . These symmetry relations reduce the number of independent components of [s] and [c] from 81 to 36. There are 9 diﬀerent ij-couples, and the same applies for the kl, thus in total 81 diﬀerent values for ijkl. Among the ij (or kl) couples, 3 are such that i = j and 6 are such that i = j. Symmetry with respect to i and j cancels 3 of the latter 6 couples, which brings to 6 instead of 9 the number of ij couples giving independent values of sijkl . The same applies for the kl couples. There remain in total 6 × 6 = 36 components of sijkl (and cijkl ) which are independent. We will see that thermodynamic arguments further reduce the number of components, which goes down to 21 because of symmetry with respect to ij and kl: sijkl = sklij and cijkl = cklij .

13.3. Contracted notation (Voigt’s notation) Because of the symmetry properties of tensor sijkl and cijkl , their expression can be simpliﬁed by replacing each couple ij (and kl) by a single subscript, denoted α for ij and β for kl, α and β ranging from 1 to 6. The correspondence is given in Table 13.1. Table 13.1: Equivalence between subscripts ij (or kl) and α (or β) ij or kl

11

22

33

2 3 and 3 2

3 1 and 1 3

1 2 and 2 1

α or β

1

2

3

4

5

6

The same simpliﬁcation makes it possible to replace the Tij and the Sij by Tα and Sα components (α ranging from 1 to 6). It is however necessary to be careful about the way these replacements are performed.

13.3.1. Stress tensor We set Tα = Tij = Tji . The tensor then takes the form: ⎛

⎞ T1 T6 T5 ⎝ T6 T2 T4 ⎠ . T5 T4 T3

(13.3)

Chapter 13 – Elasticity

265

13.3.2. Strain tensor We set: Sα = Sij

if i = j

and

Sα = Sij + Sji

if i = j.

(13.4)

The strain tensor thus has the form: ⎛ ⎞ S1 S6 /2 S5 /2 ⎝ S6 /2 S2 S4 /2 ⎠ . S5 /2 S4 /2 S3 The contracted form makes it possible to represent these two tensors in the form of column vectors with six components, Tα and Sα . We will see in the following section that the beneﬁt of using diﬀerent relations to go over from the 2-subscript notation to the single subscript notation is that the column vectors Sα and Tα are connected by a matrix relation: Sα = sαβ Tβ , and conversely Tα = cαβ Sβ .

13.3.3. Compliance tensor and stiﬀness tensor This section shows how to go over from tensors sijkl and cijkl to their simpliﬁed form sαβ and cαβ respectively. We start out by evaluating S1 = S11 = s11kl Tkl as a function of the Tα , deﬁned in Section 13.3.1: S1 = s1111 T1 + s1122 T2 + s1133 T3 + (s1123 + s1132 )T4 + (s1131 + s1113 )T5 + (s1112 + s1121 )T6 . Using the symmetry of the sijkl (Sect. 13.2.2), we set s11 = s1111 ,

s12 = s1122 ,

s13 = s1133 ,

s14 = 2s1123 ,

s15 = 2s1131 ,

s16 = 2s1112 .

We can now write: S1 = s1α Tα . The same argument applies to S2 and S3 . Now we evaluate S23 and S32 , and then add them: S23 = s2311 T1 + s2322 T2 + s2333 T3 + (s2323 + s2332 )T4 + (s2331 + s2313 )T5 + (s2312 + s2321 )T6 , S32 = s3211 T1 + s3222 T2 + s3233 T3 + (s3223 + s3232 )T4 + (s3231 + s3213 )T5 + (s3212 + s3221 )T6 . Since we set S4 = S23 + S32 , we can write: S4 = s4α Tα if we set:

s41 = 2s2311 ,

s42 = 2s2322 ,

s43 = 2s2333 ,

s44 = 4s2323 ,

s55 = 4s3131 ,

s66 = 4s1212 .

266

Symmetry and Physical Properties of Crystals

Thus we can write: Sα = sαβ Tβ providing we set: sαβ = sijkl sαβ = 2 sijkl

for α and β equal to 1, 2 or 3 (i = j and k = l), when either of the two subscripts α or β is equal to 1, 2 or 3 and the other one is equal to 4, 5 or 6, for α and β equal to 4, 5 or 6.

sαβ = 4 sijkl

We can summarize the above results by splitting Table 13.2, consisting of 9 × 9 coeﬃcients sijkl , into 9 tables with 3 rows and 3 columns each. Table 13.2: Splitting the 9×9 table of components sijkl into a set of 3×3 tables ij kl

11

22

33

23

31

12

32

13

21

11 22

I

II

III

IV

V

VI

VII

VIII

IX

33 23 31 12 32 13 21 The (6×6) matrix of coeﬃcients sαβ is obtained by superimposing and adding the sectors of the third large column to the sectors of the second large column, and then performing the same operation (superimposing, then adding) for the second and third large rows thus obtained. We ﬁnally obtain the condensed Table 13.3. Now we ﬁnd the relations between components cijkl and cαβ that allow writing Tα = cαβ Sβ . By deﬁnition, Tα = Tij = Tji , and relation (13.1b) has the form: Tα = Tij = cij11 S11 + cij22 S22 + cij33 S33 + cij23 S23 + cij32 S32 + cij31 S31 + cij13 S13 + cij12 S12 + cij21 S21 .

Chapter 13 – Elasticity

267

Table 13.3: Condensed form of the table of components sαβ α

1 2

β

3

4 5

6

1 2

I

II + III

3 4

V + VI

5

IV + VII

+

6

VIII + IX

Because of the symmetry with respect to k and l of components cijkl : Tα = Tij = cij11 S11 + cij22 S22 + cij33 S33 + cij23 (S23 + S32 ) + cij31 (S31 + S13 ) + cij12 (S12 + S21 ) and, taking into account the deﬁnition (13.4) of the Sα : Tα = cαβ Sβ if we set cαβ = cijkl . The table of the cαβ is now obtained starting from the table of cijkl by simply canceling the sectors that form the third large column and the third large row (Tab. 13.4). The components cαβ and sαβ each form a square 6 × 6 matrix. Table 13.4: Condensed form of the table of stiﬀness components cαβ . The gray areas are canceled. α β

1 2 3

4 5 6

I

II

IV

V

1 2 3 4 5 6

268

Symmetry and Physical Properties of Crystals

13.3.4. Relation between the compliance and stiﬀness tensors Using the simpliﬁed notation we just introduced, the generalized Hooke’s law can be written in the following matrix form: Sα = sαβ Tβ , Tα = cαβ Sβ . These relations show that matrices sαβ and cαβ , which we note here s and c, are mutually inverse: sc = E where E is the identity matrix. To calculate the stiﬀness components cαβ starting from the compliance components sαβ , it is suﬃcient to invert the compliance matrix, and vice versa. To conclude, the simpliﬁed notation we just introduced allows representing the stress → strain (and conversely strain → stress) relation by a matrix relation where the rank-2 tensors (stress and strain) become six-component column vectors, and the rank-4 tensors (compliance and stiﬀness) become 6 × 6 square matrices. Matrices s and c represent a simpliﬁed form of tensors sijkl and cijkl , expressed in a given coordinate system. If we want to know the expression of these matrices in another coordinate system, we have to revert to the four-subscript components of tensors sijkl and cijkl , then perform the change in axis system on these components (Eq. (13.2)), and ﬁnally revert again to the contracted form of the new components sijkl and cijkl thus obtained.

13.4. Energy of a strained solid Consider a small volume of crystal which, before deformation, has the shape of a rectangle parallelepiped. Choose a reference system consisting of orthonormal axes Ox1 x2 x3 , parallel to its sides, with lengths respectively Δx1 , Δx2 and Δx3 (Fig. 13.3). We submit it to a stress, described by the tensor Tkl which induces the strain Sij . Then we increase this deformation by a small quantity dSij . We now show that the elementary work of the stress forces during this change in deformation has the form δW = Tij dSij ΔV if ΔV is the volume of the parallelepiped. After deformation, the faces of the parallelepiped are not exactly rectangles with the same area any more, but, since the deformations are assumed to be very small, we can consider that the change in area of the faces is negligible and that the faces remain perpendicular to the coordinate axes. If the parallelepiped had been only translated without undergoing a strain, the work of the stress forces would be zero since the forces acting on two opposite faces are equal and have opposite directions. Thus the work is due only to the relative displacement of one face with respect to the other. We may

Chapter 13 – Elasticity

269

therefore, for calculation purposes, assume that the three parallelepiped faces which go through the origin remained ﬁxed, and that the work is due to the displacement of the three opposite faces. Consider the face perpendicular to axis Ox1 . It gets displaced because of the components dS11 , dS21 and dS31 of tensor dSij , which represent the relative deformation of a segment parallel to Ox1 . Term dS11 describes a displacement of this face parallel to Ox1 by Δx1 dS11 (Fig. 13.3a). During this displacement, only the component T11 of the stress tensor performs work, equal to T11 Δx2 Δx3 Δx1 dS11 = T11 dS11 ΔV . The strain component dS21 leads to a displacement of this face parallel to Ox2 by Δx1 dS21 (Fig. 13.3b), and only the component T21 performs work, equal to T21 Δx2 Δx3 Δx1 dS21 = T21 dS21 ΔV . In the same way, the strain dS31 leads to a displacement parallel to Ox3 of the face, and only the component T31 does work, equal to T31 dS31 ΔV . x3

x3

x3 O

O

x2

x2

x1 x1

x1dS11

x2

x1

x2

(a)

x1dS21

(b)

Figure 13.3: (a) Displacement parallel to Ox 1 of the face perpendicular to Ox 1 of the rectangle parallelepiped under the inﬂuence of component dS 11 of the strain tensor; (b) displacement parallel to Ox 2 of the same face under the inﬂuence of component dS 21 of the strain tensor The total work of the forces acting on the faces perpendicular to Ox1 is therefore: δW1 = Ti1 dSi1 ΔV. We would obtain in the same way the works δW2 and δW3 of the forces acting respectively on the faces perpendicular to Ox2 and Ox3 : δW2 = Ti2 dSi2 ΔV,

δW3 = Ti3 dSi3 ΔV.

The total work δW per unit volume of the material is then equal to: δW = (δW1 + δW2 + δW3 )/ΔV

or

δW = Tij dSij

(13.5)

or, in detailed form: δW = T11 dS11 + T22 dS22 + T33 dS33 + T23 dS23 + T32 dS32 + T31 dS31 + T13 dS13 + T12 dS12 + T21 dS21 .

270

Symmetry and Physical Properties of Crystals

Using relations (13.3) and (13.4) which deﬁne the Tα and the Sα components, we see that: δW = Tα dSα and, since Tα = cαβ Sβ , we can write the above relation in the form: δW = cαβ Sβ dSα . The work we just calculated is reversible work, because a small variation in strain with all of its components dSα equal and opposite to the above variation would take the system back to its initial state. The variation dF in the free energy F = U − ΘS per unit volume is such that: dF = dU − ΘdS − SdΘ = δW + δQ − ΘdS − SdΘ where S it the entropy and Θ the absolute temperature. For a reversible transformation: δQrev = ΘdS

and

dF = δWrev − SdΘ

so that dF = cαβ Sβ dSα − SdΘ. We deduce that: cαβ

(13.6)

∂ 2 F ∂ 2 F = = = cβα . ∂Sβ ∂Sα Θ ∂Sα ∂Sβ Θ

The cαβ are thus the stiﬀness coeﬃcients at constant temperature, and this relation shows that the matrix of cαβ coeﬃcients is symmetric. Therefore, the stiﬀness tensor cijkl is symmetric with respect to its two subscript groups ij and kl: cijkl = cklij . A similar argument using the thermodynamic function Φ, the Gibbs potential or free enthalpy, such that Φ = U − ΘS − Tα Sα , provides the same results for the compliance tensor. We have dΦ = −SdΘ − Sα dTα = −SdΘ − sαβ Tβ dTα and sαβ = −

∂ 2 Φ ∂ 2 Φ = − = sβα . ∂Tβ ∂Tα Θ ∂Tα ∂Tβ Θ

The sαβ are the compliance components at constant temperature and furthermore: or sijkl = sklij . sαβ = sβα These relations bring down to 21 the maximum number of independent components of the elastic and stiﬀness tensors.

Chapter 13 – Elasticity

271

The variation in free energy dF at constant temperature (dΘ = 0) takes the form, using (13.6): dF = cαα Sα dSα + cαβ (Sα dSβ + Sβ dSα ) α

=

αβ=23,31,12

cαα Sα dSα +

α

cαβ d(Sα Sβ ).

αβ=23,31,12

We obtain after integration: F=

1 α

=

2

cαα Sα2 +

cαβ Sα Sβ

αβ=23,31,12

1 1 cαα Sα2 + cαβ Sα Sβ . 2 α 2 α=β

Thus the elastic free energy per unit volume of a strained solid is given by: F =

1 cαβ Sα Sβ . 2

The above derivations were made using the expression of elementary work δW = Tα dSα . They could also have been made using the unsimpliﬁed forms of the tensors, δW = Tij dSij . We would then have obtained cijkl = cklij and sijkl = sklij , and for the free energy: F =

1 cijkl Sij Skl . 2

13.5. Eﬀect of crystal symmetry on the form of the elastic tensor We will use the direct inspection method (Sect. 9.6.2) to determine the number of independent components of the elastic (or stiﬀness) tensor for some point groups. The results for all point groups are collected in Tables 13.5a and 13.5b. Because the matrices sαβ and cαβ are symmetric, the part of the matrix deduced by symmetry is not represented. We recall that, in order to use the direct inspection method or the coordinate system change formula, we must revert to the four-subscript tensor notation.

272

Symmetry and Physical Properties of Crystals

Table 13.5a: Form of the matrices representing the compliance and stiﬀness tensors for the various point groups Triclinic

Monoclinic 2 Ox 2 m Ox 2

0 0 0

0 0 0 0

2 Ox 3 m Ox 3

0

Orthorhombic

0 0 0 0 0 0 0 0 0 0 0 0

Tetragonal

0 0 0 0 0 0 0 0 0 0

4 – 4 4/m

422 4mm – 42m 4/mmm

Equal components Components with equal absolute values but opposite signs

0 0 0 0 0 0 0 0

0 0 0 0 0 0 0 0 0 0 0 0

Chapter 13 – Elasticity

273

Table 13.5b: Form of the matrices representing the compliance and stiﬀness tensors for the various point groups Rhombohedral

3 – 3

0 0 0 0 0 0

32 3m – 3m

* Hexagonal

0 0 0 0 0

0 0 0 0

*

0 0 0 0 0 0 0 0 0 0 0 0

* Cubic

0 0 0 0 0 0 0 0 0 0 0 0

Isotropic

0 0 0 0 0 0 0 0 0 * 0 0 * 0

* Equal components Components with equal absolute values but opposite signs For s : value twice that of the component shown as a full circle to which it is connected For c : value equal to the component shown as a full circle to which it is connected

*

For s : 2(s11 – s12) For c : 1/2(c11 – c12)

274

Symmetry and Physical Properties of Crystals

13.5.1. Center of symmetry Tensors [s] and [c] being even-rank tensors, the existence or non-existence of a center of symmetry among the point symmetry operations of the crystal does not alter the number of independent components of these tensors (see Sect. 9.6.3). Thus, the number of independent components for these tensors is the same for all point groups of a given Laue class.

13.5.2. Groups 2, m and 2/m We choose axis Ox3 parallel to the 2-fold axis. Rotating the coordinate system by π around the 2-fold axis transforms components x1 , x2 , x3 of a vector into components x1 , x2 , x3 such that: x1 = −x1 ,

x2 = −x2 ,

x3 = x3 .

We deduce that the components sijkl whose subscripts i, j, k, l contain an odd total number of 1 and 2’s and, consequently, an odd number of 3’s, are zero. The tensors [s] and [c] shown in their condensed form {sαβ } or {cαβ } reduce to: 0 0 0 0 0 0 0 0

We obtain the same result by considering group m and axis Ox3 perpendicular to the mirror. The symmetry operation acting on the coordinate system changes the components x1 , x2 , x3 of a vector into components x1 , x2 , x3 such that: x1 = x1 ,

x2 = x2 ,

x3 = −x3 ,

so that any component of sijkl (or cijkl ) involving an odd number of 3’s is zero. This result is also valid for group 2/m, as expected since adding a mirror perpendicular to the 2-fold axis does not reduce the number of non-zero coefﬁcients. It is no surprise to obtain the same result for groups 2, m and 2/m since they belong to the same Laue class.

13.5.3. Groups 222, mmm and mm2 These three groups, which belong to the same Laue class, have the same number of independent coeﬃcients, and we will only consider group 222. It has three mutually perpendicular 2-fold axes, which we choose as the axes Ox1 , Ox2 and Ox3 . We use the results of the preceding section for the 2-fold axis parallel to Ox3 , and we add the symmetry operation associated to the 2-fold

Chapter 13 – Elasticity

275

axis parallel to Ox1 , a rotation by π of the coordinate system around Ox1 . This operation transforms the components x1 , x2 , x3 of a vector into components x1 , x2 , x3 such that x1 = x1 ,

x2 = −x2 ,

x3 = −x3 .

All components involving an odd total number of subscripts equal to 1 are zero. We need not consider the action of the third 2-fold axis, because its existence results from the existence of the two others. We therefore obtain the following matrix: 0 0 0 0 0 0 0 0 0 0 0 0

13.5.4. Groups 422, 4mm and 4/m mm Each of these groups belongs to the same Laue class and can be deduced from one of the above by replacing a 2-fold axis with a 4-fold axis. For these three groups, axis Ox3 is chosen parallel to the 4-fold axis. This substitution adds a symmetry operation, the rotation by π/2 around Ox3 . This operation, performed on the axis system, transforms components x1 , x2 , x3 of a vector into components x1 , x2 , x3 such that: x1 = x2 ,

x2 = −x1 ,

x3 = x3 .

We deduce that: s1111 = s2222 ,

s1133 = s2233

and s1313 = s2323 .

We ﬁnally obtain the following matrix, where lines connecting some dots indicate that the corresponding coeﬃcients are equal: 0 0 0 0 0 0 0 0 0 0 0

This result is also valid for group ¯42m, which belongs to the same Laue class.

276

Symmetry and Physical Properties of Crystals

13.5.5. Cubic system The least symmetric among the cubic groups is group 23. It has three orthogonal 2-fold axes parallel to the cube sides, and four 3-fold axes parallel to its major diagonals. We can therefore start from the number of independent coeﬃcients determined for group 222 in a system of axes parallel to the 2-fold axes, and add a 3-fold axis, for example the axis parallel to direction [111]. A rotation by 2π/3 around this 3-fold axis, performed on the axis system, transforms the components x1 , x2 , x3 of a vector into components x1 , x2 , x3 such that: x1 = x2 ,

x2 = x3 ,

x3 = x1 .

We deduce that: s1111 = s2222 = s3333

and also s1122 = s2233 = s3311 etc.

We ﬁnally obtain the following matrix: 0 0 0 0 0 0 0 0 0 0 0 0

We then check that the additional symmetries in the other cubic groups bring no further simpliﬁcation. Thus only 3 independent coeﬃcients are involved in describing the elasticity of cubic crystals. The order of magnitude of the sαβ is some 10−11 m2 N−1 , that of the cαβ some 1011 N m−2 . Some numerical values of components sαβ and cαβ are given in Tables 13.6a and 13.6b respectively.

13.6. Isotropic materials We saw, in the introduction to this chapter, that only 2 coeﬃcients are required to describe the elastic properties of isotropic materials: Young’s modulus E, and Poisson’s ratio ν. Here we will establish the connection between these coeﬃcients E and ν and the components of the compliance and stiﬀness tensors. The compliance tensor (as well as the stiﬀness tensor) of an isotropic material must be invariant under any change in coordinate system. A simple way of expressing this condition is to start from tensor sijkl for a cubic material, and to perform any change in the coordinate system (for example a rotation by π/4

Chapter 13 – Elasticity

277

Table 13.6a: Numerical values of the compliance coeﬃcients sαβ for some materials (unit: 10−11 m2 N−1 ) 11

12

44

1.5

−0.63

1.32

0.77

−0.22

1.26

2.29

−0.47

7.85

Co

6/mmm 0.47

−0.23

Ti

6/mmm 0.97

−0.47

SiC

6/mmm 0.21

−0.037 0.59

−0.017 0.18

Crystal Cu Si NaCl

P.G. ¯ m3m ¯ m3m ¯ m3m

13

33

1,32

−0.07

0.32

2.15

−0.18

0.69

14

1.10

−0.46

3.45

−0.21

Al2 O3

6mm ¯3m

0.24

−0.07

0.7

−0.038 0.22

0.049

LiNbO3

3m

0.57

−0.09

1.67

−0.15

0.49

−0.1

Quartz (SiO2 )

32

1.17

−0.08

1.72

−0.12

0.97

−0.39

KDP

¯42m

1.49

0.18

7.69

−0.39

1.97

ZnS

66

0.85

16.7

Table 13.6b: Numerical values of the stiﬀness coeﬃcients cαβ for some materials (unit: 1011 N m−2 ) 11

12

44

13

33

1.69

1.22

0.75

1.65

0.64

0.79

0.49

0.13

0.13

Co

6/mmm 3.07

1.65

0.75

1.03

3.58

Ti

6/mmm

1.6

0.9

0.46

0.66

1.81

SiC

6/mmm

5

1

1.7

0.6

5.6

ZnS Al2 O3

6mm ¯3m

1.24

0.6

0.29

0.46

1.4

4.95

1.6

1.46

1.15

4.97

−0.23

LiNbO3

3m

2.03

0.53

0.6

0.75

2.45

0.09

Quartz (SiO2 )

32

0.87

0.07

0.58

0.12

1.06

0.18

KDP

¯42m

0.71

−0.05

0.13

0.13

0.56

Crystal Cu Si NaCl

P.G. m¯3m m¯3m m¯3m

14

66

0.06

278

Symmetry and Physical Properties of Crystals

around a 4-fold axis parallel to one of the axes Ox1 , Ox2 or Ox3 ). This must leave all the tensor coeﬃcients unchanged (Exercise 13.2). We thus obtain the result that, for an isotropic material, the three independent components of the compliance and stiﬀness tensors which characterize the cubic system are connected by the following relations: s44 = 2(s11 − s12 ), c44 =

1 2 (c11

(13.7a)

− c12 ).

(13.7b)

This is of course valid whatever the orthonormal coordinate system used. There are thus only 2 independent elastic components for isotropic solids. They are expressed as a function of E and ν in the following section. We note here that cubic materials are diﬀerent from isotropic materials as far as elastic properties are concerned. This is a general result for all physical properties represented by rank-4 crystals. In contrast, for the properties represented by rank-2 tensors, cubic materials behave as isotropic (Sect. 10.5.5). The deviation from isotropy of the elastic properties of cubic materials can be evaluated by comparing the values of c44 and 12 (c11 − c12 ), or the values of s44 and 2(s11 − s12 ).

13.6.1. Expressing components sαβ as a function of E and ν Consider a tensile specimen of an isotropic material, undergoing an elongation under the inﬂuence of a uniaxial stress T . We choose Ox1 parallel to the axis of the specimen and to the stress (Fig. 13.1). The strain is obtained through the generalized Hooke’s law: ⎞ ⎛ ⎞⎛ ⎞ ⎛ ⎞ ⎛ 0 0 s11 s12 s12 0 T S1 s11 T ⎟ ⎜ ⎜ S2 ⎟ ⎜ s12 s11 s12 0 ⎟ ⎜ 0 0 ⎟ ⎟ ⎜ ⎟ ⎜ 0 ⎟ ⎜ s12 T ⎟ ⎜ ⎟ ⎜ 0 ⎟ ⎜ s12 T ⎟ ⎜ S3 ⎟ ⎜ s12 s12 s11 0 0 0 ⎟ ⎜ ⎟⎜ ⎟. ⎜ ⎟=⎜ ⎟ ⎜ ⎜ S4 ⎟ = ⎜ 0 ⎟ ⎜ 0 ⎟ 0 0 s44 0 ⎟ ⎜ ⎟⎜ 0 ⎟ ⎜ 0 ⎟ ⎜ ⎠ ⎝ ⎝ S5 ⎠ ⎝ 0 ⎠ ⎝ 0 0 0 s44 0 0 ⎠ 0 S6

0

0

0

0

0

s44

0

0

Also, s44 = 2(s11 − s12 ) according to (13.7a). The bar thus undergoes a relative elongation S1 = Δ/ = s11 T , and we deduce that s11 = 1/E where E is Young’s modulus for the material. Along with this elongation, the bar undergoes the same deformation in the two directions perpendicular to the stress: S2 = S3 = s12 T . From the deﬁnition of Poisson’s ratio ν, as given in the introduction, we see that: s12 = −ν s11 so that s12 = −

ν . E

Chapter 13 – Elasticity

279

Hence: s44 = 2

ν 1 + E E

=

2(1 + ν) . E

The shear (or rigidity) modulus G is deﬁned as the reciprocal of s44 , i.e. as the ratio of a shear stress and the corresponding shear strain, so that: G=

E 1 . = c44 = s44 2(1 + ν)

13.6.2. Stiﬀness components. Lamé coeﬃcients For isotropic materials, the stiﬀness components are not much used in the form of the cαβ . It is customary to use the Lamé coeﬃcients, λ and μ, deﬁned as follows: c44 = μ and c12 = λ and, using (13.7b): c11 = 2c44 + c12 = λ + 2μ. The stiﬀness tensor can thus be written as: ⎛ λ + 2μ λ λ ⎜ λ λ + 2μ λ ⎜ ⎜ λ λ λ + 2μ ⎜ ⎜ 0 0 0 ⎜ ⎝ 0 0 0 0 0 0

0 0 0 μ 0 0

0 0 0 0 μ 0

0 0 0 0 0 μ

⎞ ⎟ ⎟ ⎟ ⎟. ⎟ ⎟ ⎠

Hooke’s generalized law (Eq. (13.1b)) now takes the form: for α = 1, 2, 3 : and for α = 4, 5, 6 :

Tα = 2μSα + λ(S1 + S2 + S3 ), Tα = μSα .

Since Sα = Sij for α = 1, 2, 3 and Sα = Sij + Sji = 2Sij for α = 4, 5, 6, these two relations can be condensed into a single one: Tij = 2μSij + λ(Trace S)δij .

13.7. Representative surface for Young’s modulus It is often valuable to ﬁnd how the length of a bar of an anisotropic material, with known but general crystallographic direction, changes when it is submitted to a uniaxial stress parallel to the bar, i.e. the equivalent of Young’s modulus for an isotropic material. We deﬁned Young’s modulus Ew in a given direction with unit vector w as the ratio between the value T of a uniaxial stress in this direction and the relative elongation Δ/|w of the material in the same direction, Ew = T /( Δ/|w ). Choosing an orthonormal axis system (Ox1 x2 x3 ) where Ox1 is parallel to vector w, the stress tensor has only one non-zero component in this coordinate

280

Symmetry and Physical Properties of Crystals

= T . The relative elongation in direction Ox is given by S , system, T11 1 11 so that: Δ = S11 = s1111 T w

where s1111 is the compliance component expressed in the axis system (Ox1 x2 x3 ). We deduce that: 1 Ew = . s1111 We thus have to calculate s1111 as a function of the independent components sijkl of the compliance tensor in the orthonormal axis system Ox1 , Ox2 and Ox3 associated to the crystallographic system. The rule for axis system change provides: s1111 = a1i a1j a1k a1l sijkl where {aij } is the transformation matrix for going over from coordinate system (Ox1 x2 x3 ) to system (Ox1 x2 x3 ). The only coeﬃcients of the matrix actually involved are the a1j , i.e. the components of the new basis vector e1 , which is none other than vector w, in the frame Ox1 x2 x3 . These are the direction cosines of w in this frame. They are noted w1 , w2 , w3 , yielding: s1111 = wi wj wk wl sijkl . The representative surface for Young’s modulus is deﬁned as the locus of the ends of vectors starting from the same origin, with lengths in a given direction w equal to the corresponding value s1111 . This surface thus represents the reciprocal of Young’s modulus for any direction of the applied uniaxial stress. Example for the cubic system: s11 = s11 w14 + w24 + w34 + s44 w22 w32 + w32 w12 + w12 w22 + 2s12 w22 w32 + w32 w12 + w12 w22 . Since w is a unit vector, we have:

2 w14 + w24 + w34 = w12 + w22 + w32 − 2 w22 w32 + w32 w12 + w12 w22 = 1 − 2 w22 w32 + w32 w12 + w12 w22

s44 2 2 w2 w3 + w32 w12 + w12 w22 . s11 = s11 − 2 s11 − s12 − 2 Thus Young’s modulus is not isotropic for cubic crystals. and

For direction [100], s11 = s11 , while for direction [111], we obtain: s11 = s11 − 2/3 (s11 − s12 − s44 /2). It can be shown that this value is extremal (Exercise 13.5). Note: in an isotropic material, s11 − s12 = s44 /2, and, as expected, 1/E = s11 for any direction.

Chapter 13 – Elasticity

281

13.8. Compressibility Two types of compressibility at constant temperature can be deﬁned depending on whether interest focuses, for a solid submitted to a pressure variation Δp, on the change in volume or on the change in length in a given direction. In either case, the pressure variation Δp induces a variation of the stress tensor ΔTij = −δij Δp which leads to a strain variation ΔSij such that: ΔSij = sijkl ΔTkl = −sijkl δkl Δp = −sijkk Δp

(13.8)

13.8.1. Bulk compressibility The bulk compressibility coeﬃcient χ at constant temperature Θ is deﬁned by:

1 ∂V χ=− . V ∂p Θ If ΔV is a small variation in the volume V of the material caused by a small pressure variation Δp at constant temperature:

1 ΔV χ=− . Δp V We saw (Sect. 12.4) that the relative volume variation is such that: ΔV = Sii V and, because of Equation (13.8): ΔV = −siikk Δp. V Thus

1 χ=− Δp

ΔV V

= siikk

i.e. the sum of the nine coeﬃcients in the ﬁrst quarter of matrix sαβ : χ = [s11 + s22 + s33 + 2(s12 + s23 + s31 )]. In the case of an isotropic material, this relation becomes: χ = 3[s11 + 2s12 ] and, since s11 = 1/E and s12 = −ν/E, we obtain:

1 − 2ν χ=3 . E

282

Symmetry and Physical Properties of Crystals

Its reciprocal K is called the bulk modulus: K=

E 1 = . χ 3(1 − 2ν)

K and χ are positive quantities, since when the pressure applied on a solid is increased, its volume decreases: ΔV /V < 0. Thus for all materials ν < 1/2. It can also be shown [1] that the Lamé coeﬃcient μ is always positive. If E is expressed as a function of μ and ν in the expression for K, we obtain: K=

2 μ(1 + ν) 3 (1 − 2ν)

whence:

1 −1 < ν < . 2 In practice, a negative value of ν is exceptional, but it was encountered [2]. For most polycrystalline metals, described as isotropic materials, ν is on the order of 0.3.

13.8.2. Linear compressibility of a bar The linear compressibility coeﬃcient at constant temperature in a given direction w of a material, βw , is deﬁned by:

1 ∂ βw = − ∂p Θ which can be written: βw = −

1

Δ Δp

=−

1 Δp

Δ

if Δp is a small pressure variation, at constant temperature, which induces a small variation in length Δ in a segment with length parallel to vector w. We saw (Eq. (12.12)) that the relative elongation of such a segment, submitted to a variation in the strain tensor ΔSij , is given by: Δ = wi wj ΔSij w and, using Equation (13.8): Δ = −wi wj sijkk Δp. w Hence the linear compressibility coeﬃcient at constant temperature is given by: βw = wi wj sijkk .

Chapter 13 – Elasticity

283

13.9. Notes on non-uniform stresses and strains We saw in Section 11.5 that it is necessary, in order to determine tensor Tij (r) in a material submitted to given stresses (Tn )Σ on its external surface Σ, to solve Equations (11.4) ∂Tij + fi = 0, (11.4) ∂xj at all points in the solid, with the boundary conditions: (Tn )Σ = (Tij )Σ (nj )Σ .

(13.9)

We must therefore determine a tensor [T ] satisfying (11.4) and (13.9). Since tensor [T ] is related to tensor [S] through Hooke’s law [T ] = [c][S], condition (11.4) leads to a condition on the derivatives of [S]. But the six components of the symmetric tensor [S] cannot take any value in the case of non-uniform strains, because they are expressed as a function of the derivatives of the three components of the displacement vector u. Consider for example the components S11 , S22 and S12 which imply functions u1 and u2 . By deﬁnition:

∂u1 ∂u2 1 ∂u1 ∂u2 S11 = S22 = S12 = + . ∂x1 ∂x2 2 ∂x2 ∂x1 We immediately see that these three quantities are not independent. The second derivative of S12 with respect to x1 and x2 has the form:

3 ∂ 3 u2 ∂ u1 1 + 2 ∂x1 ∂x22 ∂x2 ∂x21 thus the half-sum of

∂ 2 S11 ∂x22

and

∂ 2 S22 . ∂x21

We must therefore have: 2

∂ 2 S11 ∂ 2 S22 ∂ 2 S12 = + . ∂x1 ∂x2 ∂x22 ∂x21

(13.10)

It can be shown that there are six such compatibility relations. Further, since the basic relation (11.4) must be veriﬁed, one way of incorporating the compatibility relations is to substitute, in these equations, the Sij by their expression as a function of the Tij , and to add condition (11.4). We then obtain six coupled equations, called the Beltrami-Michell equations. They can usually not be solved analytically, and their solution is obtained numerically. Another way of translating Equation (11.4) is to replace in this equation the stresses by their expression as a function of the Sij , and then to express the Sij as a function of the derivatives of displacement u. The calculation is easy in the isotropic case.

284

Symmetry and Physical Properties of Crystals

Relation (11.4) for i = 1 can be written, in the isotropic case: ∂T1j + f1 = 0 ∂xj

∂T1 ∂T6 ∂T5 + + + f1 = 0. ∂x1 ∂x2 ∂x3

or

(13.11)

Hooke’s law Tα = cαβ Sβ can we written, using the Lamé coeﬃcients (Sect. 13.6.2), as: T1 = 2μS1 + λ(S1 + S2 + S3 ), T5 = μS5 , T6 = μS6 and Equation (13.11) becomes:

∂S1 ∂S6 ∂S5 ∂S1 ∂S2 ∂S3 μ 2 +λ + f1 = 0. + + + + ∂x1 ∂x2 ∂x3 ∂x1 ∂x1 ∂x1 Also (Eq. (12.10)): 1 Sij = 2

∂uj ∂ui + ∂xj ∂xi

(13.12)

.

Since, from Equation (13.4), S5 = S13 + S31 and S6 = S12 + S21 , S5 =

∂u1 ∂u3 + ∂x3 ∂x1

and

S6 =

∂u1 ∂u2 + . ∂x2 ∂x1

Equation (13.12) thus becomes:

2 ∂ 2 u2 ∂ 2 u1 ∂ 2 u3 ∂ u1 ∂ 2 u1 + + + μ 2 2 + ∂x2 ∂x1 ∂x3 ∂x1 ∂x1 ∂x2 ∂x23

2 2 2 2 ∂ u2 ∂ u3 ∂ u1 + f1 = 0. + + +λ ∂x1 ∂x2 ∂x1 ∂x3 ∂x21 Reorganizing the terms, we obtain: 2

2 ∂ 2 u2 ∂ 2 u3 ∂ u1 ∂ u1 ∂ 2 u1 ∂ 2 u1 + (λ + μ) + f1 = 0 μ + + + + ∂x1 ∂x2 ∂x1 ∂x3 ∂x21 ∂x22 ∂x23 ∂x21 and

μ

∂ 2 u1 ∂ 2 u1 ∂ 2 u1 + + ∂x21 ∂x22 ∂x23

+ (λ + μ)

∂ ∂u1 ∂u2 ∂u3 + + + f1 = 0 ∂x1 ∂x1 ∂x2 ∂x3

so that

∂ (div u) + f1 = 0. ∂x1 We would obtain similar relations for i = 2 and i = 3 in (11.4), so that ﬁnally: μΔu1 + (λ + μ)

μΔui + (λ + μ)

∂ (div u) + fi = 0. ∂xi

The three above relations can be collected into a single vector equation: (λ + μ)grad(div u) + μΔu + f = 0 This is Navier’s equation.

Chapter 13 – Elasticity

285

To determine the strains in the solid, we must then take into account the boundary conditions on u. In a few simple cases, the solution is analytical, but in most cases it has to be determined numerically.

13.10. Exercises Exercise 13.1 Determine the form of the elasticity tensor of a crystal with point group ¯43m by using that for a crystal with point group ¯42m given in Table 13.5a. Express it in an orthonormal axis system (Ox1 x2 x3 ) parallel to the basis vectors a, b and c of the cubic unit cell. Exercise 13.2 Consider a cubic crystal, to which an orthonormal axis system parallel to the basis vectors of the cubic unit cell is associated. 1.

It is submitted to a uniform uniaxial stress T in the [100] direction. Calculate the relative elongation in the direction of the applied stress.

2.

The uniaxial stress is now applied in the direction [110]. Calculate the relative elongation in the direction of the applied stress.

3.

If the material was isotropic, the results obtained in (1) and (2) would have to be identical. Deduce the relation which exists between the elastic coeﬃcients s11 , s12 and s44 in an isotropic material.

Exercise 13.3 A small crystal sample with volume v of tin (point group 4/m mm) is submitted to a hydrostatic stress p with value 107 N m−2 . Calculate the resulting relative variation in volume. The form of the matrix {sαβ } for this group is given in Table 13.5a, and its elements, expressed in units of 10−11 m2 N−1 , are s11 = 1.85

s12 = −0.99

s13 = −0.25

s33 = 1.18

s44 = 5.7

s66 = 13.5.

Exercise 13.4 Show that the relative variation in volume of a crystal with cubic symmetry, submitted to a uniaxial stress T , is independent of the direction of the stress and is expressed by (s11 + 2s12 )T . Exercise 13.5 Show that Young’s modulus for a cubic material is maximum in the direction [111] in all cases where s11 − s12 − s44 /2 is positive.

286

Symmetry and Physical Properties of Crystals

Exercise 13.6 A crystal of lead telluride PbTe, with point group m¯3m, is submitted to a uniform uniaxial tensile stress, with intensity 108 N m−2 , perpendicular to a (110) surface. The resulting strains are the following: a relative increase in length of 24 × 10−4 in the direction of the uniaxial stress [110], relative decreases in length along directions [001] and [1¯10], with values 6 × 10−5 and 15 × 10−4 respectively. Determine the values of the elastic coeﬃcients of PbTe. Exercise 13.7 A cubic crystal with lattice parameter a is submitted to a uniform uniaxial stress T , parallel to direction [111]. 1.

Determine the stress tensor in an orthonormal axis system (Ox1 x2 x3 ) parallel to the basis vectors of the cubic unit cell.

2.

Deduce the resulting strain tensor, in the orthonormal axis system linked to the basis vectors of the cubic unit cell.

3.

Show that the cubic unit cell becomes a rhombohedral unit cell. Calculate the lattice parameters (a = b = c and α = β = γ = π/2 − ε) as a function of the uniaxial stress T and of the elastic coeﬃcients sαβ .

Exercise 13.8 Consider test specimens made of copper, with point group m¯3m, in the shape of rectangle parallelepipeds with length L and square cross section, with side . The values are L = 5 mm, = 1 mm, and the compliance tensor components of copper are: s11 = 1.49×10−11 m2 N−1 , s12 = −0.63×10−11 m2 N−1 , s44 = 1.33 × 10−11 m2 N−1 . B

A

T

C D x

L

O x B’ A’

x

C’ D’

Assume the experimental conditions are such that the stresses to which the specimens are submitted are uniform.

Chapter 13 – Elasticity

287

1.

The ﬁrst specimen is cut so that its faces are all {100} type. The uniaxial compressive stress T is applied onto the square faces ABCD and A B C D (ﬁgure above). Determine the variation in length ΔL of the specimen, and the variation Δ of the sides of the section, for T = 109 N m−2 .

2.

Consider a second specimen, with the same dimensions as the ﬁrst one, with faces now having the following crystallographic orientations: faces ABCD and A B C D are (110) faces, faces ABB A and DCC D are (001) faces and faces ADD A and BCC B are (¯ 110) faces. The uniaxial compressive stress is applied on faces ABCD and A B C D . Determine the shape taken by the specimen, and its new dimensions.

288

Symmetry and Physical Properties of Crystals

Complement 13C. Plastic deformation and crystal defects Throughout this book, the assumption is made, for simplicity’s sake, that the crystal is perfect and has inﬁnite extension. The latter condition is obviously not to be taken literally, but the assumption of crystal perfection is also most questionable. Actually, it is only through tremendous eﬀorts that crystals of silicon are manufactured (see Complement 1C) with no defect of one kind – the linear defects called dislocations which will be discussed below. Other defects, called point defects (vacancies and interstitials) are present even in these extraordinarily good crystals, because thermodynamics requires them at equilibrium. When it comes to the discussion of X-ray or neutron diﬀraction by crystals, an introductory, geometrical treatment invokes a perfect and inﬁnite crystal in order to make the reciprocal lattice (Sect. 3.2) consist of point-like nodes. Nevertheless a discussion of the scattering mechanism and scattered intensity leads to the condition that, for the experimental results to be reasonably simple to analyze (“kinematical approximation”), the crystal must be small and imperfect. And an essential physical property of metals, mechanical ductility, is directly linked to dislocations. The macroscopic strain produced by a stress, for example in a tensile test, disappears once the applied stress is removed if the strain is small enough: this is the elastic deformation range. Under a larger stress, part of the distortion remains after the stress is removed. This is plastic deformation, and obviously it is vital for metal shaping to produce permanent eﬀects, hence in all technical activities. In terms of the macroscopic stress-strain diagram, the plastic regime starts where the curve deviates from the linear initial part (Sect. 13.1). The mechanism of plastic deformation was suggested in the 1930s to be the motion and multiplication of crystal defects called dislocation lines, or for short dislocations. This postulate was required to remove the paradox associated with the fact that plastic deformation occurs for stresses much smaller than predicted from the cohesive energy for a homogeneous crystal with no singularity. The existence of dislocations was indeed conﬁrmed through direct observation when the electron microscope was developed, and they were explored in great detail also with several other techniques, notably the X-ray imaging techniques called “diﬀraction topographic methods” or Bragg-diﬀraction imaging. A dislocation can be envisaged as the result of i) performing in an initially perfect crystal a cut ending along a line (the dislocation line); ii) moving one lip of the cut with respect to the other: the displacement deﬁnes the Burgers vector b; iii) adding or removing some perfect crystal material to ﬁll the gap or remove the overlap; iv) gluing the material together. The Burgers vector must be a lattice translation in order to allow the displaced parts to match, and it is usually, for thermodynamic reasons, the shortest lattice translation possible.

Chapter 13 – Elasticity

289 b u

v u

b v

(a)

(b)

Figure 13C.1: (a) An edge dislocation: schematic representation of the atomic planes. The Burgers vector is perpendicular to the dislocation line uv. (b) A screw dislocation. The line uv and the Burgers vector are parallel. Figure 13C.1 shows the two pure situations: in (a), the dislocation line uv is perpendicular to the Burgers vector b; this is an edge dislocation, and the plane containing the line and the Burgers vector is called the glide plane. Figure 13C.1b shows the situation where the Burgers vector b is parallel to the line uv, deﬁning a screw dislocation. In reality, dislocations usually have mixed character, i.e. their Burgers vector lies at an angle to the dislocation line. As Figure 13C.1 suggests, the lattice planes are distorted in the vicinity of the dislocation. The distortion decreases with increasing distance from the core (the center) of the dislocation. The visibility of dislocations in the electron microscope and in the Bragg-diﬀraction imaging techniques is due to the strain ﬁeld: the region with inhomogeneous distortion diﬀracts diﬀerently from the perfect-crystal matrix surrounding it. The simplest case of plastic deformation through the motion of a dislocation is illustrated in Figure 13C.2, which suggests how one part of the crystal will have moved by one Burgers vector when the dislocation line has moved across the crystal. The hatched area generated by the dislocation line is called the glide plane. Dislocations interact with one another through their stress ﬁeld. This leads to a preferential arrangement of dislocations into two-dimensional boundaries (subgrain boundaries), separating regions with slightly diﬀerent orientations (typically minutes of arc). There are other defects in crystals than these line (one-dimensional) defects. They can be classiﬁed according to their geometry as point, or zero-dimensional, defects (vacancies, interstitials); plane, or two-dimensional defects (twin boundaries, stacking faults), or three-dimensional (voids, precipitates). These defects also interact with dislocations, and consequently aﬀect the plastic deformation process, leading to hardening (e.g. precipitation hardening or work hardening) when dislocation displacements are hampered. Dislocations also play an important role in the mechanism of crystal growth.

290

Symmetry and Physical Properties of Crystals

T

–T

(b)

(a) b

T v u –T

T

b

(d) –T

(c)

b

T u

v

(f)

–T

(e)

Figure 13C.2: Schematic illustration of elastic and plastic deformation processes. (a) and (c) are identical and show an initial, strain-free state. (b) is the result of elastic deformation. (d) shows the plastic deformation stage in which an edge dislocation uv, which Burgers vector b, moves to the right in its glide plane. (e) shows the plastic deformation stage in which a screw dislocation, with the same Burgers vector b, moves toward the back of the ﬁgure. (f) is the plastically deformed state after the dislocation in (d) or (e) has moved across the sample. The density of dislocations in crystals is expressed as their total length per unit volume, hence as cm . cm−3 or cm−2 . It varies from zero in the perfect single crystals of silicon made for the production of microelectronic chips, to typically 1011 cm−2 in deformed metals.

Further reading D. Hull, D.J. Bacon, Introduction to Dislocations, 5th edn. (Elsevier, 2011) H. Föll, website on crystal defects (2001) http://www.tf.uni-kiel.de/matwis/amat/mw1 ge/index.html

Chapter 13 – Elasticity

291

References [1] D. Calecki, Physique des milieux continus, vol. 1, Mécanique et thermodynamique (Hermann, Paris, 2007) [2] A. Yeganeh-Haerl, D.J. Weidner, J.B. Parise, Science 257, 650–652 (1992)

Chapter 14

Elastic waves in crystals This chapter introduces an important application of the elasticity tensors: the propagation in crystals of acoustic waves, the velocity of which depends directly on the stiﬀness tensor. The end of this chapter discusses brieﬂy the relation between this macroscopic property and atom vibrations.

14.1. Introduction In the preceding chapter, we investigated the elastic behavior of crystalline solids submitted to static forces. These forces induce strains, which are connected to them through the elastic coeﬃcients. These coeﬃcients were ﬁrst measured using static approaches, which yield limited accuracy because the induced strains are very small. We will see in this chapter that, if the material is submitted to a strain wave, the velocity at which this wave propagates depends on the stiﬀness coeﬃcients of the material. These propagation velocities can be measured with an accuracy much higher than through static measurements. Therefore the stiﬀness coeﬃcients, from which the elastic coeﬃcients are deduced, are nowadays measured using techniques based on elastic wave propagation velocity. The elastic waves are excited in the crystal by transducers made from piezoelectric crystals (Sect. 15.3.6): when excited by a sinusoidal electric ﬁeld, they create a sinusoidal strain wave which is transmitted by contact to the crystal under investigation. In Sections 14.2, 14.3 and 14.4, the crystal is, as in all preceding chapters starting from Chapter 9, considered as a continuous medium. This assumption only holds as long as the wavelength of the elastic waves is much larger than the dimensions of the crystal’s unit cell. The frequency range used in applications is that of sound and ultrasound waves, gathered under the denomination of acoustic waves. Their frequency varies from 1 kHz to about 10 GHz, so that, considering the order of magnitude of the propagation velocity of sound in crystal materials (some 103 m s−1 ), the condition is satisﬁed. Nevertheless, it is worthwhile understanding the connection between this macroscopic approach and the microscopic treatment which directly takes into consideration

© Springer Science+Business Media Dordrecht 2014 C. Malgrange et al., Symmetry and Physical Properties of Crystals, DOI 10.1007/978-94-017-8993-6_14

293

294

Symmetry and Physical Properties of Crystals

the atomic arrangement and the binding forces between atoms. This is done in the last section, using a highly simpliﬁed model (a linear chain of equidistant identical atoms) which however provides insight into the behavior of a real crystal (three-dimensional unit cell, and several atoms per unit cell). These results are important, and they are given without derivation in Section 14.5.3.

14.2. Plane elastic waves Consider a solid submitted to an elastic perturbation, and a small volume element dv of this solid centered at a point with position vector r0 at rest. Its position at time t becomes: r(t) = r0 + u(r0 , t)

(14.1)

where u(r0 , t) is the displacement vector. The resultant F of the forces applied to this element dv is, using (11.3), such that:

∂Tij + fi dv Fi dv = ∂xj and, applying Newton’s second law:

∂Tij ∂ 2 xi + fi dv = (ρdv) 2 ∂xj ∂t

(14.2)

where ρ is the mass per unit volume of the solid. If the bulk forces f are zero or considered to be negligible, as we assume in the rest of this chapter, then: ∂ 2 xi ∂Tij =ρ 2 . (14.3) ∂xj ∂t Using (14.1),

and (14.3) becomes:

∂ 2 ui ∂ 2 xi = 2 ∂t ∂t2 ∂Tij ∂ 2 ui =ρ 2 . ∂xj ∂t

(14.4)

We can relate the components Tij to the partial derivatives of the components ui with respect to the position variables. The stress tensor Tij is related to the strain tensor Skl through the stiﬀness tensor cijkl (Eq. (13.1b)). Furthermore (Eq. (12.10)),

1 ∂uk ∂ul + . Skl = 2 ∂xl ∂xk We thus obtain: Tij = cijkl Sk

1 = cijkl 2

∂ul ∂uk + ∂xl ∂xk

Chapter 14 – Elastic waves in crystals and

∂Tij 1 = cijkl ∂xj 2

295

∂ 2 uk ∂ 2 ul + ∂xj ∂xl ∂xj ∂xk

.

The two terms on the right-hand side of this equation are equal since we sum over j, k and l. We can thus write:

2 ∂ ul ∂Tij = cijkl ∂xj ∂xj ∂xk and Equation (14.4) becomes:

cijkl

∂ 2 ul ∂xj ∂xk

=ρ

∂ 2 ui . ∂t2

(14.5)

We now show that the general solution to this equation has the form: s · r s · r + Be G t + . u(r, t) = AeF t − v v For simplicity, we restrict consideration to the ﬁrst term in this solution: s j xj s · r = AeF t − . u(r, t) = AeF t − v v This is the equation of a plane wave propagating along a direction parallel to unit vector s, with components si , because sj xj , hence the phase of the wave, is constant over any plane perpendicular to vector s (Fig. 14.1). If we consider any point M with coordinates xj , the plane P perpendicular to s and going through M intersects axis O, parallel to s, at H the projection of M and of all points of the plane onto O. For all points M in the plane, OM · s = xj sj = OH = and we can write:

s · r = AeF t − , (14.6) u(r, t) = AeF t − v v a plane wave whose wave planes move parallel to s, at velocity v. Unit vector e, whose components are noted ei , is called the polarization vector of the wave.

M r O s

H

P

Figure 14.1: Plane P perpendicular to unit vector s. This plane is the locus of points M for which s · r = s · OM = OH = const = .

296

Symmetry and Physical Properties of Crystals

Consider the form (14.6) of the displacement, and calculate its derivatives with respect to time and space, in order to substitute them into (14.5): ∂ 2 ui = Aei F , ∂t2 ∂ul sk = −Ael F ∂xk v

and

sj sk ∂ 2 ul = Ael 2 F ∂xj ∂xk v

where F and F are respectively the ﬁrst and second derivatives of F (w) with respect to w. Equation (14.5) becomes: cijkl el so that

sj sk F = ρei F v2

cijkl sj sk el = ρ v 2 ei .

(14.7)

Γil = cijkl sj sk

(14.8)

We set: and Equation (14.7) can be written as: Γil el = ρv 2 ei .

(14.9)

This equation shows that vector e is an eigenvector of matrix {Γil }, and that the eigenvalue associated to it is equal to ρv 2 . The terms in matrix {Γil } relate a vector to another vector. They are therefore the coeﬃcients of a rank-2 tensor [Γ] (Sect. 9.4.2), called the Christoﬀel tensor. This tensor is symmetric, since: Γli = cljki sj sk = ckilj sj sk because cαβ = cβα (Sect. 13.4). Also, since tensor cijkl is symmetric with respect to i and j and with respect to k and l (Sect. 13.2.2): Γli = cikjl sk sj

and

Γli = Γil .

Because matrix Γ is real and symmetric, it has three orthogonal eigenvectors. The eigenvalues are the solutions of the following equation, called the Christoffel equation: Γ11 − ρv 2 Γ12 Γ13 2 = 0. Γ12 Γ22 − ρv Γ23 2 Γ13 Γ23 Γ33 − ρv Once the eigenvalues are known, it is easy to deduce the eigenvectors, i.e. the polarization vectors of the corresponding elastic wave.

Chapter 14 – Elastic waves in crystals

297

Expanding the expression of one of the coeﬃcients Γil , for example Γ11 : Γ11 = c1111 s21 + c1121 s1 s2 + c1131 s1 s3 + c1211 s2 s1 + c1221 s22 + c1231 s2 s3 + c1311 s3 s1 + c1321 s3 s2 + c1331 s23 . Hence, using for the cijkl the two-subscript notation with α and β: Γ11 = c11 s21 + c66 s22 + c55 s23 + 2 (c16 s1 s2 + c15 s3 s1 + c56 s2 s3 ) . The other Γij coeﬃcients can be calculated in the same way, and the result is given in the form of Table 14.1. Each row of the table gives, for the coeﬃcient Γil indicated at the beginning of the row, the elastic coeﬃcients to be associated to each of the six terms s21 , s22 , s23 , s2 s3 , s3 s1 , s1 s2 in the sum. Table 14.1: Table showing the form of the components Γij of Christoffel’s tensor s21

s22

s23

s2 s3

s3 s1

s1 s2

Γ11

c11

c66

c55

2 c56

2 c15

2 c16

Γ22

c66

c22

c44

2 c24

2 c46

2 c26

Γ33

c55

c44

c33

2 c34

2 c35

2 c45

Γ23

c56

c24

c34

c44 +c23

c45 +c36

c46 +c25

Γ31

c15

c46

c35

c45 +c36

c13 +c55

c14 +c56

Γ12

c16

c26

c45

c25 +c46

c56 +c14

c12 +c66

In conclusion, three elastic waves can propagate in a crystal. The propagation velocity vj of each of these waves j, the phase velocity, is deduced from the corresponding eigenvalue ξj = ρ vj2 of the matrix {Γil } associated with the Christoﬀel tensor. The corresponding polarization vector ej is the eigenvector associated to ξj . The three polarization vectors are mutually orthogonal.

14.3. Application to a cubic crystal The stiﬀness matrix of a cubic crystal is expressed, in a system of axes parallel to the basis vectors of the crystal lattice: ⎛ ⎞ 0 0 c11 c12 c12 0 ⎜ c12 c11 c12 0 0 0 ⎟ ⎜ ⎟ ⎜ c12 c12 c11 0 0 0 ⎟ ⎟. c=⎜ ⎜ 0 0 ⎟ 0 0 c44 0 ⎜ ⎟ ⎝ 0 0 0 0 c44 0 ⎠ 0 0 0 0 0 c44

298

Symmetry and Physical Properties of Crystals

The Christoﬀel tensor coeﬃcients can then be expressed as: Γ12 = (c44 + c12 ) s1 s2 Γ11 = c11 s21 + c44 s22 + s23 2 2 2 Γ22 = c11 s2 + c44 s3 + s1 Γ23 = (c44 + c12 ) s2 s3 2 2 2 Γ31 = (c44 + c12 ) s3 s1 . Γ33 = c11 s3 + c44 s1 + s2 Their value depends on the propagation direction s of the plane wave. The next two sections deal with two special cases.

14.3.1. Propagation of a plane wave along direction [100] s1 = 1,

In this case:

s2 = s3 = 0.

The only non-zero coeﬃcients of the Christoﬀel tensor are thus: Γ11 = c11 ,

Γ22 = c44 ,

Γ33 = c44 .

The propagation velocities must satisfy equation: c11 − ρv 2 0 0 2 − ρv 0 0 c 44 0 0 c44 − ρv 2 the obvious solutions of which are: v1 =

= 0,

c11 ρ

with eigenvector (1, 0, 0) so that the wave is longitudinal (Fig. 14.2a), and c44 v2 = v3 = ρ for which the eigenvectors are vectors of the subspace formed by vectors (0, 1, 0) and (0, 0, 1), in other words all vectors perpendicular to vector s: the wave is transverse (Fig. 14.2b). x3

x3

O x1

e1

s

e2

O

x2

s

x2

x1

(a)

(b)

Figure 14.2: Polarization vectors for waves propagating in a cubic crystal along direction [100]: (a) longitudinal wave; (b) transverse wave

Chapter 14 – Elastic waves in crystals

299

14.3.2. Propagation along direction [110] 1 s1 = s2 = √ , 2

In this case:

s3 = 0.

The only non-zero values of Christoﬀel’s tensor are: Γ11 =

c11 + c44 , 2

Γ22 =

c11 + c44 , 2

Γ33 = c44 ,

Γ12 =

The propagation velocities must satisfy equation: c +c c44 + c12 11 44 − ρv 2 0 2 2 + c + c c c 44 12 11 44 0 − ρv 2 2 2 0 0 c44 − ρv 2

c44 + c12 . 2

= 0.

Vector (0, 0, 1)is an obvious eigenvector, and the associated propagation velocity is v3 = c44 /ρ (Fig. 14.3). This wave is transverse. The eigenvalues v1 and v2 are solutions of:

2

c11 + c44 c44 + c12 2 2 − ρv − =0 2 2

hence v1 =

2c44 + c12 + c11 2ρ

and

v2 =

c11 − c12 . 2ρ

It is easy to show that√the polarization vector of the wave with propagation velocity v1 is e1 = (1/ 2)(1, 1, 0), so that the wave is longitudinal because e1 is parallel to s. √ The polarization vector of the wave with propagation velocity v2 is e2 = (1/ 2)(1, −1, 0), so that this is a transverse wave. x3 e3 e2

O s

x1

e1

x2

Figure 14.3: Polarization vectors for a wave propagating in a cubic crystal along direction [110]: (e1 ) and the wave is longitudinal, (e2 , e3 ) and the waves are transverse Notes: 1.

We found longitudinal and transverse waves to be the solutions in the two above cases, but these are very special cases. For a general propagation direction, the vibration modes are neither purely longitudinal

300

Symmetry and Physical Properties of Crystals nor purely transverse. The wave whose polarization vector is closest to the propagation direction s (i.e. for which the angle between e and s is smallest) is called quasi-longitudinal and the two other waves are called quasi-transverse.

2.

The velocity v is a phase velocity. In the case of a sine wave

k u(r, t) = Ae cos(ωt − k · r) = Ae cos(ωt − ks · r) = Ae cos ω t − s · r , ω the phase velocity v is equal to ω/k. We found above that the value of v does not depend on the angular frequency ω. Thus the crystal material is non-dispersive for acoustic waves. However it is anisotropic, and this velocity depends on the direction of vector k since the Christoﬀel tensor [Γ] depends on it. The group velocity vg , with components (vg )i = ∂ω/∂ki , which is the propagation direction of energy, is generally no more parallel to the wave vector.

3.

We showed (Sect. 12.4) that the relative volume variation of a deformed solid is equal to the trace of the strain tensor: ∂ui = div u. ∂xi In the special case of a transverse wave, it is easy to show that div u = 0. If one of the axes, for example Ox1 , is chosen parallel to the propagation vector s, the only non-zero components of u are u2 and u3 and, since they do not depend on x2 and x3 , div u = 0 and propagation occurs with no change in volume. In contrast, propagation of any other waves, for which div u = 0, entails expansion and compression regions in the solid.

14.4. Isotropic solid case This case is easily deduced from the propagation in a cubic crystal, by considering a general direction and using relation (13.7b) which connects the stiﬀness coeﬃcients of an isotropic material: c44 =

c11 − c12 . 2

Consider for example propagation direction [100] in a cubic material. From the results of Section 14.3.1, one longitudinal wave, with propagation velocity v , and transverse waves, with propagation velocity vt , can propagate, with c11 c44 vt = . v = ρ ρ Using the Lamé coeﬃcients λ and μ (see Sect. 13.6.2) such that: λ + 2μ = c11

μ = c44 ,

Chapter 14 – Elastic waves in crystals

301

the velocities of the longitudinal and transverse waves, v and vt respectively, become: λ + 2μ μ v = and vt = . ρ ρ The ratio of these longitudinal and transverse wave velocities is: λ 2μ + λ v = 2+ . = vt μ μ This ratio is always larger than 1. Hence, in an isotropic material, the longitudinal elastic waves propagate faster than the transverse elastic waves. Of course the same results would be obtained using the results of Section 14.3.2, derived for a propagation direction parallel to [110].

14.5. Microscopic approach – Crystal lattice dynamics Till now, we considered the crystal to be a continuous and homogeneous medium. It is worthwhile understanding how this macroscopic approach can be connected to a microscopic description involving the vibrations of the atoms. At equilibrium, the average interatomic distance in a crystal is the one which minimizes the crystal’s energy. If an atom is moved away from its equilibrium position, it is submitted by its neighbors to restoring forces which cause it to oscillate around its equilibrium position. These oscillations are transmitted to the neighboring atoms, thus creating within the solid an elastic wave which propagates in the crystal. The full treatment of atomic vibrations in a crystal, crystal lattice dynamics, involves no major diﬃculty, but it implies a rather cumbersome algebraic approach, with a wealth of subscripts, which is beyond the scope of this book. Nevertheless, the main characteristics of the results can be deduced from the simple model of a one-dimensional crystal, i.e. a linear chain of atoms. We will start out by working out the case of a chain of identical atoms, then that of a chain containing two types of atoms. These two examples provide the essential results of the full treatment.

14.5.1. Linear chain of identical atoms Consider a linear chain of N identical atoms, with mass M , the same distance a apart (Fig. 14.4). The atom displacements in the chain are assumed to be small enough that a series expansion to ﬁrst order of the energy with respect to the displacement be valid, which is equivalent to considering a harmonic potential. Furthermore, we assume that the forces between atoms are restricted to forces between nearest neighbors. We can thus imagine a chain of atoms connected by springs with the same coeﬃcient K.

302

Symmetry and Physical Properties of Crystals A0

a

A1

Aj –1

Aj

Aj +1

AN – 2

AN –1 x

O

Figure 14.4: One-dimensional chain consisting of a single kind of atoms, with mass M, at the same distance a from one another The force between two atoms is a restoring force proportional to the diﬀerence in distance between the displaced and the undisplaced atoms. There are N atoms, denoted as A0 , A1 , . . ., Aj , . . ., AN −1 . Atom j is, at equilibrium, at position x0j = ja, and, if it is displaced by uj , it is submitted to two forces, with respective algebraic values (Fig. 14.5): (a) K(uj−1 − uj ), the force exerted by atom j − 1, (b) K(uj+1 − uj ), the force exerted by atom j + 1. Their resultant Fj is: Fj = K(uj+1 + uj−1 − 2uj ). A0 O

Aj –1

a

Aj

Aj +1 x

uj –1

uj

uj +1

Figure 14.5: Displacement of the atoms in the one-dimensional chain. The positions of the atoms at equilibrium are the empty circles and the positions after displacement are the full circles. Applying Newton’s second law to the j-th atom, we obtain the equation for its motion: ∂ 2 uj (14.10) M 2 = K(uj+1 + uj−1 − 2uj ) ∂t thus altogether N equations for the N atoms. This system of N equations simpliﬁes considerably if we seek a solution where all the atoms have a sinusoidal movement with the same amplitude, the displacement being in the form of a plane monochromatic wave. For atom j: uj = A cos(kx0j − ωt) = A cos(kja − ωt) = A [exp i(kja − ωt)]

(14.11)

where means “real part of”. We set vj = exp i(kja − ωt), and we seek vj as a solution of Equation (14.10), which becomes ∂ 2 vj (14.12) M 2 = K(vj+1 + vj−1 − 2vj ). ∂t

Chapter 14 – Elastic waves in crystals

303

Since this equation is linear, uj will be a solution if vj is. We obtain: ∂ 2 vj = −ω 2 vj , ∂t2 vj−1 = e−ika vj

and

vj+1 = eika vj .

Equation (14.12) becomes: K K [2 − (e−ika + eika )] = 2 (1 − cos ka) M M

K ka ω 2 = 4 sin2 M 2 ω2 =

and

ω (k) = 2

ka K sin . M 2

(14.13)

The ω(k) curve is called the dispersion curve. It is periodic, with period equal to 2π/a (Fig. 14.6). Furthermore it is symmetric. It is therefore suﬃcient to consider half a period, for example 0 < k < π/a. K 2 — M

–– a

0

– a

k

Figure 14.6: Dispersion curve ω(k) of a linear chain consisting of identical equidistant atoms with mass M We notice that the dispersion relation (14.13) does not depend on j. Thus the N equations (14.12) lead to a single dispersion relation, which justiﬁes the choice we made of a sinusoidal displacement wave (14.11). However, we started out from N coupled oscillator equations, which means that if a single atom starts vibrating, it will not continue vibrating with the same amplitude. It transfers energy to its neighbors in a complicated way. The sine-wave solutions we sought are collective oscillations, uncoupled (independent) from one another, called the normal modes. Each mode corresponds to one well-deﬁned value of k and one well-deﬁned value of ω; hence, in the language of quantum physics, it is a stationary state. The number of normal modes is equal to the

304

Symmetry and Physical Properties of Crystals

number of equations we started from, N . If we want each atom to have the same environment, we must assume that N is very large, and that the chain is closed on itself (Born and Von Karman’s periodic boundary conditions). This implies that atom j coincides with atom j + N , so that uj = uj+N , and eikN a = 1, so that: kN a = 2pπ with p an integer 2pπ . Na There are thus N values of k in one period 2π/a, for example between −π/a and π/a. and

k=

We now look at two limiting cases: k very small, i.e. k π/a and k = π/a. If k π/a, then λ a. The wavelength is very large compared to the interatomic distance, and we expect to retrieve the results obtained when we assume the medium to be continuous. We notice that, in this case, many atoms have almost identical motions, and thus the discrete character of the chain vanishes. Equation (14.13) becomes ω ≈ ka K/M and the phase velocity vϕ = ω/k is: ω K =a . k M It is independent of k. The crystal is non-dispersive for such waves, in agreement with the result of the macroscopic treatment, and the velocity of the acoustic waves va is: K va = a . (14.14) M If k = π/a, Equation (14.11) becomes uj = A cos (ωt − jπ). There is no propagation any more, and two neighboring atoms, j and j + 1, vibrate in phase opposition. The maximum angular frequency ωm of the associated waves is given by: K ωm = 2 M whence a cutoﬀ frequency fc = ωm /2π which can be related to the above acoustic wave velocity va determined in (14.14): va 1 K fc = = . (14.15) π M πa The results obtained with this extremely simple model can be generalized to the case of a real monoatomic crystal. It can be shown that there are three dispersion curves for one propagation direction of the wave. Each curve is

Chapter 14 – Elastic waves in crystals

305

associated to one of the polarization vectors determined at the beginning of this chapter, and its slope at origin is the associated propagation velocity. This one-dimensional model can be used to check that the frequency range of acoustic waves does correspond to the linear part of these dispersion curves. The order of magnitude of the cutoﬀ frequency deﬁned above (Eq. 14.15) can be calculated from the order of magnitude of the acoustic wave velocity va , some 103 m s−1 : we choose arbitrarily 3 × 103 m s−1 . If we assume an interatomic distance on the order of 2 Å, we obtain a cutoﬀ frequency on the order of 5 THz. The acoustic wave range does not extend beyond a few GHz, it is thus indeed in the linear part of the dispersion curve.

14.5.2. Linear chain with two diﬀerent atoms We now consider a linear chain of atoms, with period a, containing two types of equidistant atoms, with mass respectively M and m (Fig. 14.7). The coordinate x0j of the j-th atom at equilibrium is x0j = ja/2. a M

m

Figure 14.7: One-dimensional chain, with period a, consisting of two types of atoms, with mass M and m, a distance a/2 apart During motion, the coordinate xj of this atom becomes: xj = j(a/2) + uj . As in the case of the monoatomic chain, we model the interaction force between nearest neighbor atoms with a harmonic restoring force, the equivalent of a spring with stiﬀness K. The force on the j-th atom is then given by: Fj = K(uj+1 − uj ) + K(uj−1 − uj ). The equations of motion are respectively M

∂ 2 uj = K(uj+1 + uj−1 − 2uj ), ∂t2

(14.16a)

for atom j with mass M , and m

∂ 2 uj+1 = K( uj+2 + uj − 2uj+1 ) ∂t2

(14.16b)

for atom j + 1 with mass m. As in the preceding case, we look for a solution having the form of a sinusoidal wave: uj = A [ei(kja/2−ωt) ]

and

uj+1 = αA [ei(k(j+1)a/2−ωt) ]

306

Symmetry and Physical Properties of Crystals

where α is the ratio of the respective displacement amplitudes of masses m and M . We obtain: −M ω 2 = K[α(eika/2 + e−ika/2 ) − 2] −mαω 2 eika/2 = K[(eika + 1) − 2αeika/2 ] so that M ω 2 = 2K [1 − α cos ka/2]

(14.17a)

2

mαω = 2K [α − cos ka/2] .

(14.17b)

From Equations (14.17a) and (14.17b): α=

2K cos(ka/2) 2K − M ω 2 . = 2K cos(ka/2) 2K − mω 2

This implies 2

2

2

(2K − mω )(2K − M ω ) = 4K cos so that mM ω 4 − 2K(m + M )ω 2 + 4K 2 sin2

2

ka 2

ka 2

= 0.

This is a second-degree equation in ω 2 , with solutions: 1/2 K(m + M ) ± (m + M )2 K 2 − 4K 2 mM sin2 (ka/2) 2 ω = mM so that ω2 =

1/2 ! K . (m + M ) ± (m + M )2 − 4mM sin2 (ka/2) mM

The ω(k) curve has two branches (Fig. 14.8). Their limiting values for k π/a and for k = π/a can be easily calculated. If k π/a, sin ka/2 ≈ ka/2 1 and we obtain: (m + M ) K and ω ≈ ka . ω ≈ 2K mM 2(m + M ) The corresponding values of α are −M/m and 1. The ﬁrst solution corresponds to point A in Figure 14.8. The atoms with masses m and M respectively vibrate in phase opposition and their center of mass is at rest (Fig. 14.9a). If the chain consists of an alternation of positive and negative ions, their motion leads to an electric polarization of the material. This gives a possibility of interacting with electromagnetic waves which leads, in particular, to wave absorption in the relevant frequency range. These frequencies happen to be those of optical electromagnetic waves. This is why this branch of the dispersion curve is called the optical branch or the optical mode.

Chapter 14 – Elastic waves in crystals

307

K(m+M) 2 ——— A mM

–– a

K 2— m

B

K 2— M

C

– a

0

k

Figure 14.8: Dispersion curve ω(k) for a periodic linear chain consisting of two types of equidistant atoms, with masses respectively M and m

(a)

(b)

Figure 14.9: Vibration modes for a periodic linear chain consisting of two types of equidistant atoms, in the approximation k π/a, so that λ 2a. For clarity, (i) we assume the vibrations to be transverse, and not longitudinal, and (ii) the wavelength is not extremely large with respect to period a. (a) Optical branch: the atoms with masses m and M respectively vibrate in phase opposition and their center of mass is at rest. (b) Acoustic branch: the two types of atoms vibrate in phase with the same amplitude.

308

Symmetry and Physical Properties of Crystals

The second solution corresponds to long wavelength acoustic waves. Both types of atoms vibrate in phase with the same amplitude (Fig. 14.9b). The material is no more dispersive (ω/k is constant) and the propagation velocity v is equal to ω/k: v=a

K . 2(m + M )

This is the equivalent of the propagation velocity of sound waves. If k = π/a, sin ka/2 = 1 and the two solutions for ω 2 are: K K and ω= 2 . ω= 2 m M The corresponding values of α are α = ∞ and α = 0. This limit corresponds to a half-wavelength equal to a, the distance between atoms of the same type. In the ﬁrst solution, mass m oscillates and mass M is at rest (point B in Fig. 14.8). It is no surprise that the frequency then depends only on mass m. In the second case, mass M oscillates and mass m is at rest (point C on Fig. 14.8).

14.5.3. Extension to the real crystal case The simpliﬁed theory we just presented makes it possible to understand the results for a real three-dimensional crystal. The dispersion curves ω(k) are then represented for a given direction of vectors k. The results are as follows: The dispersion curves feature 3 acoustic modes, analogous to the single acoustic mode of the linear chain. The slopes at origin of these modes are equal to the propagation velocities of the acoustic waves determined under the macroscopic theory. If two velocities are the same in some propagation direction, there are only two acoustic modes, one of them being degenerate. If the crystal contains one single atom per primitive unit cell, there are only acoustic modes. If the crystal contains two atoms per unit cell, there are, additionally, three optical modes, the properties of which are similar to those of the optical mode of the linear chain. The optical modes can also be degenerate. If the crystal contains p atoms per unit cell, there are 3p modes, 3 of which are acoustic modes and 3(p − 1) are optical modes. In all cases, the linear parts of the acoustic modes, near the origin of the dispersion curves, are compatible with the assumptions of continuity and homogeneity of the material, and consistent with the macroscopic results on the propagation of acoustic waves.

Chapter 14 – Elastic waves in crystals

309

14.6. Exercises Exercise 14.1 Consider the propagation of elastic waves in a crystal with mass per unit volume ρ. 1.

The crystal is monoclinic, and c is the basis vector parallel to the 2-fold axis or perpendicular to the mirror. We consider an elastic wave with wave-vector parallel to direction [001]. (a) Write down Christoﬀel’s matrix. (b) Determine the velocity and the polarization of the waves which propagate in the crystal.

2.

Same questions for an orthorhombic crystal, and a propagation direction parallel to direction [001].

3.

Same questions for a crystal having an n-fold rotation axis, with n > 2, and propagation direction parallel to direction [001].

4.

The crystal is hexagonal. The propagation direction is a general direction in the plane perpendicular to c. Show that a wave with polarization parallel to c, therefore transverse, propagates.

Exercise 14.2 The components of the stiﬀness tensor of diamond are to be determined from the measurement of the propagation velocities of elastic waves. Diamond is cubic and its mass per unit volume is 3.51 g cm−3 . 1.

Calculate the propagation velocity of longitudinal waves along direction [100].

2.

Calculate the propagation velocities along direction [111].

3.

The propagation velocities were measured in a diamond crystal for both of the above wave-vector directions. The results are as follows: For k parallel to [100]: velocity of transverse waves: vt = 11,196 m s−1 . For k parallel to direction [111]: velocity of the longitudinal wave: vl = 14,490 m s−1 , velocity of the transverse waves: vt = 13,239 m s−1 . Determine the components of the stiﬀness tensor of diamond.

Exercise 14.3 Consider a tetragonal crystal with point group 422. Determine the propagation velocity of elastic waves with wave-vector parallel to direction [110] in this crystal.

Chapter 15

Crystal thermodynamics. Piezoelectricity The aim of this chapter is to introduce crossed eﬀects, in which quantities related to diﬀerent areas of physics (thermal, mechanical, electrical) are connected through thermodynamics. It then deals with an example which is important through its many diverse applications: piezoelectricity. The mechanical properties of crystals were studied in Chapters 11, 12 and 13. We brieﬂy recall below their electrical and thermal properties. Usually, these properties are studied independently of one another. For example, the application of stress leads to a deformation of the material, the magnitude of which depends on the value of its elastic coeﬃcients. In a similar way, an electric ﬁeld applied to a crystal induces an electrical induction which depends on the dielectric permittivity of the material. In both of these examples, the physical quantities involved are of the same nature, or, to put it another way, belong to the same domain or area (mechanical and electrical respectively), and the eﬀects involved are called principal eﬀects. This is no more the case when, applying a variation in temperature (thermal constraint), we measure a variation in polarization (an electrical quantity, the phenomenon of pyroelectricity) or a strain (a mechanical quantity, the phenomenon of thermal expansion). The response does not belong to the same area, and the eﬀects involved are called crossed eﬀects. Thus, the response of a crystal to a constraint may have several aspects and imply various physical properties. The aim of this chapter is to examine the various responses of crystals to a given constraint. To introduce these eﬀects and the connections between them, it is necessary to assume the crystal to be in an overall thermodynamic state deﬁned by one parameter in each of the thermal, mechanical and electrical domains. This will be done in the ﬁrst section, and will make it possible to introduce various crossed eﬀects. We will then study more speciﬁcally two special crossed eﬀects, viz. the properties of pyroelectricity (Sect. 15.2) and piezoelectricity (Sect. 15.3) featured by some crystals.

© Springer Science+Business Media Dordrecht 2014 C. Malgrange et al., Symmetry and Physical Properties of Crystals, DOI 10.1007/978-94-017-8993-6_15

311

312

Symmetry and Physical Properties of Crystals

15.1. Crystal thermodynamics 15.1.1. Conjugate variables Mechanical quantities We have seen that, under the eﬀect of a stress represented by a tensor [T ], a material undergoes a strain [S] such that [S] = [s][T ] Sij = sijkl Tkl

or

and, in contracted notation (Sect. 13.3): Sα = sαβ Tβ .

(15.1)

[s] is the tensor of elastic compliances, which connects the response [S] of the crystal to the constraint [T ]. In a similar way, the stress is related to the strain by the tensor of elastic stiﬀnesses [c] according to the relation [T ] = [c][S] or

Tij = cijkl Skl

and in contracted notation Tα = cαβ Sβ . During a change in the strain dSij , the work δW received by unit volume of the system1 is given by Equation (13.5), i.e. δW = Tij dSij

or

δW = Tα dSα .

(15.2)

Tensors [S] and [T ] are the conjugate quantities, or conjugate variables, in the mechanical domain. Electrical quantities When submitted to an electric ﬁeld E, a material polarizes, and its polarization P, the dipole moment per unit volume, is P = ε0 [χ]E, where [χ] is the electrical susceptibility tensor. The electrical induction D is such that D = ε0 E + P = ε0 ([E] + [χ])E = ε0 [ε]E

(15.3)

1. Here we assume, for simplicity’s sake, that the stress and the strain are homogeneous. If this were not the case, we would have to write δW = Tij dSij dv, where the integral is performed over unit volume.

Chapter 15 – Crystal thermodynamics. Piezoelectricity

313

which can also be written as Di = ε0 εij Ej .

(15.4)

ε0 is the permittivity of vacuum, the value of which, in the international system (SI) of units, is 10−9 /36π = 8.8 × 10−12 , and [ε] is the electrical permittivity tensor which connects the response D of the crystal to the electric ﬁeld E. Relation (15.4) can be inverted by introducing the impermeability tensor [η], the inverse of the relative electrical permittivity tensor [ε]: Ei = ηij

Dj . εo

During a variation in induction dD, the work received by unit volume of the system is (see e.g. [1])2 δW = Ei dDi = E · dD.

(15.5)

D and E are the conjugate quantities in the electrical domain. Relation (15.3) must be altered for some materials which additionally feature a polarization P0 , the spontaneous polarization, in the absence of an electrical ﬁeld. For these materials: D = P0 + ε0 [ε]E

(15.6)

so that, in zero ﬁeld, D = P0 . These materials are called pyroelectric because, as we will see, this intrinsic polarization varies with temperature. They can only belong to some crystal classes3 (Sect. 9.5.2). Thermal quantities If we apply a reversible change in temperature dΘ to unit volume of a material, it receives per unit volume a quantity of heat δQrev : δQrev = Cexp dΘ 2. The exact form given by Landau and Lifshitz in [1] is δW = Ei dDi dv, where the integral must be taken over the whole volume, including vacuum if the dielectric does not occupy all of the space between conductors. We therefore assume here that the material ﬁlls all the space between conductors, and that E and D are homogeneous in the material. This makes it possible to refer to the work per unit volume of the material. 3. We recall that a crystallographic class includes all crystals with a given point group.

314

Symmetry and Physical Properties of Crystals

where Cexp is the heat capacity per unit volume of the material under the conditions of the experiment (e.g. at constant volume or at constant pressure). The quantity of heat is not one of the variables deﬁning the state of a system, and δQ is not a total diﬀerential. We must consider the entropy of the system S, deﬁned by its variation dS during a reversible transformation where the temperature changes from Θ to Θ + dΘ: dS =

Cexp δQrev = dΘ. Θ Θ

(15.7)

Entropy S and temperature Θ are the conjugate variables of the thermal domain.

15.1.2. Independent variables Consider a system with unit volume, deﬁned by three quantities, each of them chosen in one of the above domains, viz. the thermal, electrical and mechanical domains. In the thermal domain, we can choose temperature Θ or entropy S, which are scalars. In the electrical domain, the electric ﬁeld E or induction D, which are vectors deﬁned by three components. And in the mechanical domain the strain tensor or the stress tensor, both symmetrical tensors with six independent components each. The state of the system is thus deﬁned in total by 10 independent variables. For clarity, we actually consider the tensor form of tensors [T ] and [S], with the two-subscript notation Tij and Sij for their coeﬃcients,4 and will thus consider 13 variables which are only quasi-independent since three of them are equal to three others (Tij = Tji and Sij = Sji for i = j). We will then revert to the contracted notation and to the 10 independent variables. When the system changes state, its internal energy per unit volume U changes by dU such that dU = ΘdS + δW where dS is the change in entropy and δW the reversible work, so that here δW = Ei dDi + Tkl dSkl and dU = ΘdS + Ei dDi + Tkl dSkl . If we are interested in the internal energy of the system, the usual choice of independent variables is the entropy S per unit volume, the three components of induction Di , and the 9 components of strain Skl . We call these variables, which appear in the diﬀerential of the various terms in dU , the thermodynamic coordinates of the system, and we denote them as xi , with index i ranging 4. This makes it possible to clearly deﬁne the transition from the two subscripts ij to the single subscript α for the new tensors which will be introduced (thermal expansion and piezoelectricity).

Chapter 15 – Crystal thermodynamics. Piezoelectricity

315

from 1 to 13. The variables Θ, Ei and Tkl are the variables conjugate to the variables xi chosen to deﬁne the system. We note Xi the quantity conjugate to the thermodynamic coordinate xi , and thus dU = Xi dxi

(15.8)

using Einstein’s convention. The conjugate quantities Xi are intensive quantities, whereas the thermodynamic coordinates are often inaccurately described as extensive quantities. The electrical induction D is in fact homogeneous to a polarization, i.e. to a dipole moment per unit volume, and the components of the strain tensor deﬁne the relative variations in length. Thus the components Di and Skl cannot be considered as extensive quantities. Nevertheless they are quasi-extensive quantities because they are the ones to be multiplied by the value of the volume when the latter is no more unity. In practice, it is often more convenient to choose as independent variables deﬁning the system the conjugate quantities Xi . We are then led to considering another thermodynamic function5 of the system, the free enthalpy or Gibbs potential G, such that G = U − ΘS − Ei Di − Tkl Skl and dG = −SdΘ − Di dEi − Skl dTkl .

(15.9)

We thus conclude that ∂G ∂G ∂G Di = − Skl = − . (15.10) S =− ∂Θ Ej ,Tmn ∂Ei Θ,(Ej ),Tmn ∂Tkl Θ,Ei ,(Tmn ) In these formulas, the indexed variables that are taken to be constant during diﬀerentiation are indicated in parentheses when all of them are constant except for the one with respect to which diﬀerentiation is performed. For example, D1 is the derivative of G with respect to E1 at constant (Ei ), Θ, Tkl , meaning that E2 , E3 , Θ and all Tkl ’s are held constant. Using the above notation, with the xi representing the thermodynamic coordinates (the variables involved in the diﬀerential element of the elementary variation in internal energy (15.8)), and Xi their respective conjugate quantities, chosen here as deﬁning the state of the system, the relations (15.9) and (15.10) respectively take on the condensed form dG = −xi dXi and

∂G xi = − . ∂Xi (Xj )

(15.11)

5. The use of various thermodynamic functions depending on the independent variables of a problem is particularly well discussed in [2].

316

Symmetry and Physical Properties of Crystals

We can make a Taylor expansion of the value of each coordinate xi as a function of its value xi (0) in the initial state. We denote as Xj (0) the values of the conjugate quantities in the initial state. We obtain ∂xi (Xj − Xj (0)) (15.12) xi − xi (0) = ∂Xj 0 j

if we restrict the Taylor expansion to its ﬁrst term. This is equivalent to considering that the ﬁrst derivatives ∂xi ∂Xj 0 are constant, or that the variations (Xj − Xj (0)) are small. This is an approximation, usually valid, which will be used in this and the following chapters. Only in the last chapter shall we show that some special eﬀets (such as electrooptical and piezo-optical eﬀects) require the inclusion of higher order terms. The same would apply for other eﬀects such as non-linear elasticity, but we will not deal with them in this book. Using Equations (15.11), relation (15.12) can be written as ∂2G (Xj − Xj (0)) xi − xi (0) = − ∂Xj ∂Xi 0 j

or xi − xi (0) = Mij (Xj − Xj (0))

(15.13)

using Einstein’s convention for subscript j (ranging from 1 to 13) and setting ∂ 2 G . (15.14) Mij = − ∂Xj ∂Xi 0 Since the order of the diﬀerentiations does not matter: Mji = Mij . We thus deﬁned a symmetrical matrix with 13 rows and 13 columns, called the physical property matrix M . Consider an initial reference state at Θ = Θ0 , without stress so that Tkl = 0, and in zero electric ﬁeld, so that Ei = 0, and a ﬁnal state where Θ = Θ0 + ΔΘ, Ei = 0, Tkl = 0. In the reference state, Ei is zero, hence, according to Equation (15.4), induction Di is also zero, except if the crystal is naturally polarized, which is the case for pyroelectric crystals (Eq. (15.6)). For the latter the reference state has a spontaneous polarization P0 at Θ0 . Since the stress tensor Tkl is zero in the reference state, so is the strain Skl . Thus, in the reference state, S = S0 , Di = 0 (except for pyroelectrics where D0 = P0 ) and Skl = 0. Thus the only thermodynamic quantity with non zero

Chapter 15 – Crystal thermodynamics. Piezoelectricity

317

value xi (0) is S0 . The 13 components of the vector xi − xi (0) are therefore S − S0 = ΔS, Dj and Smn . A slightly more detailed presentation of Equations (15.13), using Einstein’s convention (Sect. 9.3.1), is the following: ∂2G ∂2G ∂2G ΔΘ − − (15.15a) E Tkl , i ∂Θ2 ∂Ei ∂Θ ∂Tkl ∂Θ ∂2G ∂2G ∂2G ΔΘ − Ei − Tkl , (15.15b) Dj = − ∂Θ∂Ej ∂Ei ∂Ej ∂Tkl ∂Ej ∂2G ∂2G ∂2G ΔΘ − Ei − Tkl . (15.15c) Smn = − ∂Θ∂Tmn ∂Ei ∂Tmn ∂Tkl ∂Tmn The partial derivatives are calculated for the reference state, assuming the variables other than those with respect to which derivation is performed to be constant. ΔS = −

Equations (15.15) connect the components of a 13-component vector y (ΔS, Dj , Smn ) to the 13 components of another vector Y (ΔΘ, Ei , Tkl ) via the physical property matrix deﬁned above in (15.14), i.e. yi = Mij Yj .

(15.16)

15.1.3. Principal eﬀects vs crossed eﬀects Some coeﬃcients of the matrix Mij are known and represent the principal eﬀects. They are the “diagonal” terms in the broad sense, which we recall below. The variation in entropy ΔS at zero electric ﬁeld Ei and stress Tkl , as a function of the variation in temperature, is C ΔQ = ΔΘ ΔS = Θ Θ where C is the heat capacity per unit volume of the material (at zero electric ﬁeld and stress). Similarly, if an electric ﬁeld Ei is applied (at zero ΔΘ and Tkl ), the induction Dj is given by Dj = εji Ei , where εji is the relative electrical permittivity tensor. We note that εij = εji since εij = −

∂2G ∂Ei ∂Ej

and the order of the derivations is irrelevant. The tensor [ε] is symmetrical. Applying a stress Tkl (at zero ΔΘ and Ei ) gives rise to a strain Smn such that Smn = smnkl Tkl . We note that smnkl = sklmn since smnkl = −

∂2G . ∂Tkl ∂Tmn

318

Symmetry and Physical Properties of Crystals

We retrieve the symmetry of tensor [s] which we already derived in Section 13.4. The non-diagonal terms correspond to the crossed eﬀects, and are pairwise equal since matrix Mij is symmetrical. Thus the system (15.15) can be rewritten as: ΔS = (C/Θ)ΔΘ + pi Ei + αkl Tkl ,

(15.17a)

Dj = pj ΔΘ + εji Ei + djkl Tkl ,

(15.17b)

Smn = αmn ΔΘ + dimn Ei + smnkl Tkl .

(15.17c)

In these expressions, we set: ∂2G ∂2G =− , ∂Ei ∂Θ ∂Θ∂Ei ∂2G ∂2G αkl = − , =− ∂Tkl ∂Θ ∂Θ∂Tkl ∂2G ∂2G =− . djkl = − ∂Tkl ∂Ej ∂Ej ∂Tkl pi = −

(15.18a) (15.18b) (15.18c)

The coeﬃcients pj (called the pyroelectric coeﬃcients) in Equation (15.17b) describe the pyroelectric eﬀect, i.e. a variation in spontaneous polarization under the inﬂuence of a change in temperature at zero stress and electric ﬁeld. We recall, from the beginning of this section, that the reference state for D in pyroelectric crystals is the spontaneous polarization P0 at the reference temperature Θ0 . The quantity Dj in Equation (15.17b) is then the component ΔPj of the variation in spontaneous polarization ΔP under the inﬂuence of the variation in temperature, i.e. ΔPj = pj ΔΘ. The same coeﬃcients describe the electrocaloric eﬀect (Eq. (15.17a)), i.e. the production of heat under the inﬂuence of an electric ﬁeld in pyroelectric crystals. The coeﬃcients αmn (Eq. (15.17c)) describe thermal expansion (strain Smn under the inﬂuence of a variation in temperature ΔΘ, with Smn = αmn ΔΘ) and also the piezocaloric eﬀect (Eq. (15.17a)), i.e. the production of heat ΔQ = ΘΔS = Θαkl Tkl under the inﬂuence of a stress Tkl . The coeﬃcients djkl (Eq. (15.17b)) describe the direct piezoelectric eﬀect, i.e. the appearance of a polarization under the inﬂuence of a stress Dj = Pj = djkl Tkl or, for pyroelectric crystals, the appearance of an additional polarization ΔPj = djkl Tkl . They also describe (Eq. (15.17c)) the appearance of a strain under the inﬂuence of an electric ﬁeld, Smn = dimn Ei . This is called the inverse piezoelectric eﬀect.

15.1.4. Summary of the various eﬀects The above results are summarized in Table 15.1. The various eﬀects are represented on Figure 15.1 by a drawing borrowed from [3].

Chapter 15 – Crystal thermodynamics. Piezoelectricity

319

Table 15.1: Table describing the physical eﬀects related to the coeﬃcients of the physical property matrix. The principal eﬀects are shaded. Thermodynamic coeﬃcients ΔΘ ΔS

Dj

Smn

Ei

Tkl

Heat capacity C/Θ

Electrocaloric eﬀect pi

Piezocaloric eﬀect αkl

Pyroelectricity pj

Electrical permittivity εji

Direct piezoelectric eﬀect djkl

Thermal expansion αmn

Inverse piezoelectric eﬀect dimn

Elasticity smnkl

ric effect p Pyroelect

Heat capacity

Thermal ex

oe

eff ec t

rm

[ T]

S

s

ic lor

e eff

ec t eff

Th erm

oe

tic

las

lec

tic

e Th

s

pansion [ ]

[ ct

]

] y [s

[ S]

it ca [ d] tic zo ec t las e E i c eff P i r t lec zoe pie t c Dire

D Inve rse

Electromechanical effects

Ele

c tr oc

Pe rm

alo

ric

eff ec tp y pie [] zoe lec t ric e ffec t [d ]

itti

vit

E

Figure 15.1: Schematic representation of the principal and crossed eﬀects (adapted from [3], by permission of Oxford University Press)

320

Symmetry and Physical Properties of Crystals

Two equilateral triangles are drawn with the same center and the same orientation. The thermodynamic coordinates (the xi , which are the entropy, electrical induction and strain) are placed at the vertices of the internal triangle (i). Their conjugate quantities (the Xi , which are the temperature, the electric ﬁeld and the stress) are placed at the vertices of the external triangle (e). The arrangement is such that two conjugate quantities are located on the same median of the triangles. The arrows indicate the paths from one quantity to another. Those connecting a quantity and its conjugate (arrow from e to i) represent the principal eﬀects. For example, the arrow connecting Θ to S (thermal domain) corresponds to a change in entropy due to a variation in temperature, i.e. the heat required to obtain a variation in temperature, and the physical quantity associated to this eﬀect is the heat capacity. The temperature vertex Θ of the external triangle can be connected to quantities from another domain in the internal triangle, viz. the electrical induction or the strain, and the associated arrows (from e to i) correspond to crossed eﬀects (pyroelectric eﬀect and thermal expansion). The straight line segments parallel to the sides of the triangle are paths from i to i or e to e. The area between two such parallel segments, such as the segment connecting Θ to E and the one connecting S to D, represent various eﬀects that couple two domains, here the thermal and the electrical domain; the various eﬀects are designated as thermoelectric.

15.1.5. Condensed representation of the physical property matrix The way we deﬁned it, the physical property matrix connects two 13-component vectors. We know that, because tensors Sij and Tij are symmetric, we can replace the nine components Sij and Tij by the 6 independent components Sα and Tα deﬁned in (13.3) and (13.4) respectively. Thus vectors yi and Yi become 10-component vectors and matrix M a 10 by 10 matrix (Fig. 15.2). The “diagonal” terms which connect the Sα and Tα are then the contracted elastic coeﬃcients sαβ . The crossed terms implying the Sα and Tα are the components diα and αβ which are deduced from components dijk and αij . We will show in Section 15.3.2 how to go over from the dijk to the diα . Let us see how we go over from the components αij of the thermal expansion tensor (equal to the piezocaloric tensor) to the contracted components αβ . If we apply a temperature variation ΔΘ at zero or constant electric ﬁeld and stress, the components of the strain tensor Smn can be written as: Smn = αmn ΔΘ, which we want to write as Sβ = αβ ΔΘ. It is clear that, for S11 , S22 and S33 , which are respectively equal to S1 , S2 and S3 , we simply set αβ = αmm . The same does not apply for β = 4, 5 or 6. For example, for β = 4, S4 = S23 + S32 = (α23 + α32 )ΔΘ = α4 ΔΘ if we set α4 = α23 + α32 .

Chapter 15 – Crystal thermodynamics. Piezoelectricity ⎛ ⎜ ⎜ ⎜ ⎜ ⎜ ⎜ ⎜ ⎜ ⎜ ⎜ ⎜ ⎜ ⎜ ⎜ ⎜ ⎝

ΔS D1 D2 D3 S1 S2 S3 S4 S5 S6

⎞

⎛

⎟ ⎜ ⎟ ⎜ ⎟ ⎜ ⎟ ⎜ ⎟ ⎜ ⎟ ⎜ ⎟ ⎜ ⎟ ⎜ ⎟=⎜ ⎟ ⎜ ⎟ ⎜ ⎟ ⎜ ⎟ ⎜ ⎟ ⎜ ⎟ ⎜ ⎠ ⎝

C T p1

p2 p3 α1 α2 α3 α4 α5 α6

p1 ε11 ε12 ε13 d11 d12 d13 d14 d15 d16

p2 ε12 ε22 ε23 d21

p3 ε13 ε23 ε33 d31

α1 d11 d21 d31 s11 s12 s13 s14 s15 s16

α2 d12 d22 d32 s12 s22

α3 d13 d23 d33 s13 s23 s33

α4 d14 d24 d34 s14 s24 s34 s44

321

α5 d15 d25 d35 s15 s25 s35 s45 s55

α6 d16 d26 d36 s16 s26 s36 s46 s56 s66

⎞⎛ ⎟⎜ ⎟⎜ ⎟⎜ ⎟⎜ ⎟⎜ ⎟⎜ ⎟⎜ ⎟⎜ ⎟⎜ ⎟⎜ ⎟⎜ ⎟⎜ ⎟⎜ ⎟⎜ ⎟⎜ ⎠⎝

ΔT E1 E2 E3 T1 T2 T3 T4 T5 T6

⎞ ⎟ ⎟ ⎟ ⎟ ⎟ ⎟ ⎟ ⎟ ⎟ ⎟ ⎟ ⎟ ⎟ ⎟ ⎟ ⎠

Figure 15.2: Physical property matrix Thus we conclude that for β = 1, 2, 3:

αβ = αmm ,

for β = 4, 5, 6:

αβ = αmn + αnm .

It is easy to check that this result remains valid for the piezocaloric eﬀect, which can be written as ΔS = αβ Tβ . In the following sections, we study more speciﬁcally two of the crossed eﬀects we just introduced, viz. pyroelectricity and piezoelectricity.

15.2. Pyroelectricity. Pyroelectric crystals Pyroelectric crystals feature a spontaneous polarization in the absence of an electric ﬁeld. They are crystals for which the centers of gravity of the positive and of the negative charges in the unit cell do not coincide. For these materials: D = P0 + ε0 [ε]E. In the absence of an applied electric ﬁeld, and at a given reference temperature Θ0 : D = P0 . This polarization is diﬃcult to evidence because the surface charges due to polarization are rapidly neutralized by free charges from the air or through conduction in the crystal. However, its variation as a function of temperature can be measured more easily, and this change (at zero electric ﬁeld and stress) ΔP = P(Θ)−P(Θ0 ) is related, according to Equation (15.17b), to the variation in temperature ΔΘ = Θ − Θ0 by ΔPi = pi ΔΘ

or

ΔP = pΔΘ.

p is a vector whose components are the pyroelectric coeﬃcients.

322

Symmetry and Physical Properties of Crystals

We showed (Sect. 9.5.2) that pyroelectricity can occur only in crystals belonging to one of the following point groups: 1, 2, 3, 4, 6, m, mm2, 3m, 4mm and 6mm. The best known pyroelectric crystal is tourmaline, whose variation in polarization with temperature was evidenced in antiquity. The materials most used in applications (especially for infrared radiation detectors) are ferroelectric materials because their pyroelectric coeﬃcients are usually higher. Ferroelectric crystals are pyroelectric crystals whose spontaneous polarization can be reversed under the inﬂuence of high enough an electric ﬁeld. These crystals generally undergo a phase change at a given temperature, called the Curie temperature Θc , above which they are no more pyroelectric. Therefore the pyroelectric coeﬃcients are usually negative in a representation where the components of the spontaneous polarization are positive, since the spontaneous polarization decreases with increasing temperature and ﬁnally disappears beyond Θc . Among the best known materials are potassium dihydrogen phosphate KH2 PO4 , usually denoted as KDP, and barium titanate BaTiO3 . The point group of KDP is mm2 (orthorhombic system) in the ferroelectric phase and ¯42m (tetragonal system) above its Curie temperature Θc equal to −150◦ C. Barium titanate has the perovskite structure (Sect. 8.2.4), with point group m¯3m (cubic system) above the Curie temperature Θc = 120◦ C. As temperature is reduced below Θc , its point group is 4mm (tetragonal system). It then undergoes more transitions, its point group becoming mm2 (orthorhombic system) at Θ = 5◦ C, then 3m (rhombohedral system) at Θ = −90◦ C. It remains ferroelectric in these three phases. Ferroelectric materials are often used in the form of ceramics, i.e. as powders submitted to compacting and sintering at high temperatures, because they are easier to manufacture than single crystals and they can be given any shape. Without special treatments, the microcrystals forming the ceramics have random relative misorientation and their polarization can take on all possible orientations. Their average polarization is then zero. To obtain a sizable polarization, the ceramic is submitted to a strong electric ﬁeld which orients the polarization of each of the domains in the grains in the direction closest to the electric ﬁeld consistent with the crystal symmetry and the grain orientation.

15.3. Piezoelectric crystals 15.3.1. Direct eﬀect and inverse eﬀect A piezoelectric crystal polarizes under the action of an applied stress (direct eﬀect) and, conversely, deforms when an electric ﬁeld is applied (inverse eﬀect). The direct eﬀect was discovered by Pierre and Jacques Curie in 1880. The inverse eﬀect was predicted the following year by Gabriel Lippman on the basis of thermodynamic considerations, and its existence immediately veriﬁed by the Curie brothers.

Chapter 15 – Crystal thermodynamics. Piezoelectricity

323

The direct piezoelectric eﬀect connects the polarization induced in the crystal P and the applied stress [T ]. This eﬀect shows up at zero electric ﬁeld, and we can write, in agreement with Equation (15.17b): Di = Pi = dijk Tjk .

(15.19)

The inverse piezoelectric eﬀect connects the quantities conjugate to [T ] and D, viz. the strain [S] and the electric ﬁeld E respectively. Equation (15.17c) shows that (15.20) Sij = dkij Ek . It is worth noticing the diﬀerence in the order of the subscripts in the piezoelectric coeﬃcients dijk for the direct and inverse eﬀects in Equations (15.19) and (15.20). This is due to the deﬁnition, in (15.18), of the coeﬃcients dijk : the ﬁrst subscript points to a diﬀerentiation of free enthalpy with respect to a component of E, while the two last ones point to diﬀerentiation with respect to a component of [T ]. The above conditions, viz. zero electric ﬁeld to describe the direct eﬀect, and zero stress to describe the inverse eﬀect, are fulﬁlled only in special geometries or for high sample symmetry. Usually, the electric and mechanical quantities are coupled, and we must consider, at constant temperature, the two coupled equations resulting from (15.17b) and (15.17c): Pj = εji Ei + djkl Tkl , Smn = dimn Ei + smnkl Tkl .

(15.21a) (15.21b)

15.3.2. Piezoelectric tensor [d] and its two-subscript notation Equation (15.19) shows that the coeﬃcients dijk connect the second-rank tensor [T ] with the vector P, a ﬁrst-rank tensor. They are therefore the coeﬃcients of a third-rank tensor (Sect. 9.4.2). The same conclusions are reached by considering Equation (15.20), where the coeﬃcients dkij connect the ﬁrst-rank tensor E to the second-rank tensor [S]. A third-rank tensor comprises 33 = 27 coeﬃcients. This number can here be reduced by taking into account the symmetry of the stress tensor, allowing the 9 coeﬃcients Tij to be replaced by the six coeﬃcients Tα (Eq. (13.3)). Suppose we apply a stress for which only the components T23 = T32 are nonzero. The resulting polarization is Pi = di23 T23 + di32 T32 = (di23 + di32 )T23 . Since we cannot distinguish di23 and di32 , we set: dijk = dikj which reduces the number of independent components of tensor [d] to 18. Using the contracted notation, we immediately see that Equation (15.19) can be written as: (15.22) Pi = diα Tα

324

Symmetry and Physical Properties of Crystals

provided we set diα = dijk

for α = 1, 2 and 3 (j = k),

(15.23a)

diα = 2dijk

for α = 4, 5, 6 (j = k).

(15.23b)

Now relation (15.22) can be written in matrix form. The components Pi form a column vector with three rows, the components Tα a column vector with six rows, and the table of coeﬃcients diα a matrix with 3 rows and 6 columns. We thus obtain ⎛ ⎞ T1 ⎛ ⎞ ⎛ ⎞ ⎜ T2 ⎟ ⎜ ⎟ d11 d12 d13 d14 d15 d16 P1 ⎜ ⎟ ⎝ P2 ⎠ = ⎝ d21 d22 d23 d24 d25 d26 ⎠ ⎜ T3 ⎟ . ⎜ T4 ⎟ ⎜ ⎟ P3 d31 d32 d33 d34 d35 d36 ⎝ T5 ⎠ T6 The inverse piezoelectric eﬀect can be written as: Sij = dkij Ek . We see that, using the deﬁnitions (15.23) of the coeﬃcients diα , and the contracted notation for tensor [S] (Eq. (13.4)), we can write: Sα = diα Ei . This relation becomes a matrix relation provided we use the matrix dT , transposed from the preceding one, i.e. dTαi = diα ⎛

or

⎜ ⎜ ⎜ ⎜ ⎜ ⎜ ⎝

S1 S2 S3 S4 S5 S6

⎞

⎛

⎟ ⎜ ⎟ ⎜ ⎟ ⎜ ⎟=⎜ ⎟ ⎜ ⎟ ⎜ ⎠ ⎝

and d11 d12 d13 d14 d15 d16

d21 d22 d23 d24 d25 d26

Sα = dTαi Ei d31 d32 d33 d34 d35 d36

⎞ ⎟⎛ ⎞ ⎟ E1 ⎟ ⎟ ⎝ E2 ⎠. ⎟ ⎟ E3 ⎠

15.3.3. Eﬀect of crystal symmetry on the form of the tensor The piezoelectric tensor, a material tensor, must be invariant under all the point symmetry operations of the crystal (Sect. 9.5.2). We remember that, in applying this principle, we must revert to the three-subscript notation of the piezoelectric tensor.

Chapter 15 – Crystal thermodynamics. Piezoelectricity

325

Centrosymmetric crystal A centrosymmetric crystal cannot be piezoelectric, since odd-rank tensors are identically zero for all crystals featuring a center of symmetry (Sect. 9.6.3). We can retrieve this result directly from Curie’s principle. The symmetry of the eﬀect (electrical polarization, with symmetry ∞m) must include the symmetry of the cause (crystal + stress). Stress is centrosymmetric. If the crystal also is centrosymmetric, the intersection of the symmetry groups of the stress and of the crystal features a center of symmetry, and this is incompatible with symmetry group ∞m. Examples of reduction in the number of non-zero coeﬃcients We can apply the direct inspection method (Sect. 9.6.2) to all crystallographic groups except for those which contain a 3-fold or 6-fold axis. For the latter, we must revert to the matrix method (Sect. 9.6.1). We give below a few examples of the use of the direct inspection method, while the result for all crystal groups is given in Table 15.2. 1.

Crystals with group 2 We choose axis Ox3 parallel to the 2-fold axis. Rotating the coordinate system by angle π around Ox3 changes the components xi of a vector into components xi such that x1 = −x1 ,

x2 = −x2 ,

x3 = x3 .

Coeﬃcients dijk transform as the product of 3 components, so that for example d111 = −d111 , and on the other hand they must be invariant in the coordinate system rotation, so that d111 = d111 , which means that d111 = 0. We understand from this example that, if the subscripts i, j and k include an even number (0 or 2) of the value 3, which implies an odd number of the set of 1’s and 2’s, dijk = 0. Reverting to the 2-subscript notation, we obtain the table ⎞ ⎛ 0 0 0 d14 d15 0 ⎝ 0 (15.24) 0 0 d24 d25 0 ⎠ . d31 d32 d33 0 0 d36 2.

Crystals with group m Let us choose Ox3 perpendicular to the mirror. The action of the mirror perpendicular to Ox3 on the coordinate system changes the components xi of a vector into components xi such that x1 = x1 ,

x2 = x2 ,

x3 = −x3 .

326

Symmetry and Physical Properties of Crystals This time the coeﬃcients dijk that contain an odd number of indices equal to 3 are zero. The tensor now has the form: ⎞ ⎛ 0 d16 d11 d12 d13 0 ⎝ d21 d22 d23 0 0 d26 ⎠ . 0 0 0 d34 d35 0 Adding a 2-fold axis perpendicular to this mirror, we check that, for the centrosymmetric group 2/m, all coeﬃcients are zero.

3.

Crystals with group 222 We again consider matrix (15.24), and now add the eﬀect of the existence of another 2-fold axis. Choosing axis Ox2 along this second 2-fold axis, the zero coeﬃcients are those containing an even number of 2’s. The tensor thus becomes: ⎞ ⎛ 0 0 0 0 d14 0 ⎝ 0 0 0 0 d25 0 ⎠ . 0 0 0 0 0 d36 The eﬀect of a third 2-fold axis would bring nothing more, since the existence of this third axis is the direct consequence of the existence of the two others. Equivalently, we can say that the generating elements of the group 222 are restricted to rotations by π around two perpendicular axes.

4.

We note that group 423, although it is not centrosymmetric, has a piezoelectric tensor that is identically zero (Exercise 15.1).

Note: a crystal belonging to a piezoelectric group does not necessarily feature a piezoelectric eﬀect. The values of the components of the piezoelectric tensor depend very much on the crystal itself, and in some cases the coeﬃcients are all zero even when measured with high sensitivity. In this respect, the piezoelectric tensor is diﬀerent from the elastic or thermal expansion tensors. Conversely, experimentally detecting a piezoelectric signal indicates beyond doubt the absence of centrosymmetry in a crystal. When possible, the piezoelectric test is therefore a valuable complement to structural diﬀraction data, for which the conclusion on the presence or absence of centrosymmetry is diﬃcult. Form of the piezoelectric tensors for all crystal groups Table 15.2 shows the non-zero coeﬃcients of the piezoelectric tensor for all crystal groups, and Table 15.3 gives some numerical values for the coeﬃcients diα , in units of 10−12 C N−1 .

Chapter 15 – Crystal thermodynamics. Piezoelectricity

327

Table 15.2: Form of the matrix representing the piezoelectric tensor for the various crystal groups Triclinic 1 Monoclinic

2 Ox 2

0 0 0

0 0

0 0 0 m Ox 2 0 0 0

222 Tetragonal 4

0

0 0

0 0 0 0 0 0 0 0 0 0 0 0 0

0 0 0 0 0 0

– 4

0 0 0 0 0 0 0 0 0 0 0

4mm

0 0 0 0 0 0 0 0 0 0 0 0 0

32 2 Ox 1

0 0 0 0 0 0 0 0 0 0 0 0 0

0 0 0 0 0

0 0 0 0 0

6

622

0 0 0 0 0 0 0 0 0 0

0 0 0 3m 0 0 0 0 m Ox 2 0 0 0

0 0 0 0 0 0

6mm

0 0 0 0 0 0 0 0 0 0 0 0 0

– 6

0 0 0 0 0 0 0 0 0 0 0 0

0 0 0 0 0

0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0

0 0 0 0 0 – 62m 0 0 0 0 m Ox 1 0 0 0 0 0 0

0 0 0 0 – 62m 0 0 0 0 0 m Ox 2 0 0 0 0 0 0

0 0 0 0 0 0 0 0 23 0 0 0 0 0 0 0 0 – 43m 0 0 0 0 0 0 0 0 Equal components Components with equal absolute values Component equal to minus twice the component shown as a full black circle to which it is connected

Cubic

432

0

mm2

0 0 0 0 0 0 0 0 0 0 0 0 0 0 0

Hexagonal

0 0 0

0 0 0 0 0 0 0 0 0 0 0 0 0 0 0

– 42m 2 Ox 1

3m m Ox 1

0 0 0 0

m Ox 3

0

0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0

3

0 0

0 0 0 0 0 0 0 0

422

Rhombohedral

2 Ox 3

0

0 Orthorhombic

0

0 0 0 0 0 0 0 0 0 but opposite signs

328

Symmetry and Physical Properties of Crystals Table 15.3: Numerical values of the piezoelectric coeﬃcients for some materials, in units 10−12 C N−1 (from [4]) KDP (¯42m)

d14

d36

1.4

23.2

d15

d22

d31

d33

74

20.77

0.86

16.23

SiO2 (32)

d11

d14

Quartz

– 2.3

– 0.67

GaAs (¯43m)

d14

LiNbO3 (3m)

– 2.7 (25◦ C) 2.63 (196◦ C) InSb (¯43m)

d14 – 2.35 (25◦ C)

15.3.4. Longitudinal piezoelectricity surface The longitudinal piezoelectricity surface is obtained by plotting, on any direction with unit vector s, a length equal to the modulus of d111 in the orthonormal set of axes (Ox1 x2 x3 ), where Ox1 is parallel to s. To represent this threedimensional surface, we perform sections by planes going through the origin. The sign of d111 is then indicated as we will see with the example below. Assume the components of the piezoelectric tensor are known in the orthonormal axis system (Ox1 x2 x3 ) associated to the crystal axes, and denoted in this set of axes as dijk . We obtain d111 from the dijk ’s through the usual rule (Sect. 9.4.1): d111 = a1i a1j a1k dijk where {aij } is the transformation matrix for going over from the set of axes (Ox1 x2 x3 ) to the set (Ox1 x2 x3 ). aij is the component parallel to axis Oxj of the unit vector parallel to Ox1 , here denoted as s. Calling si the components of s in the axis system (Ox1 x2 x3 ), we then have d111 = si sj sk dijk .

(15.25)

We can interpret Equation (15.25) as follows. Assume the experimental conditions are such that, when applying a uniaxial stress at constant temperature to a piezoelectric crystal, the electric ﬁeld in the crystal is zero (Fig. 15.3). According to (15.19), we would obtain a polarization Pi = dijk Tjk . In a set of axes (Ox1 x2 x3 ) such that axis Ox1 is parallel to the uniaxial stress, the latter

Chapter 15 – Crystal thermodynamics. Piezoelectricity

329

x3 T

x’1

s

x2

x1

Figure 15.3: Schematic illustration of the meaning of longitudinal piezoelectricity, a measure of the polarization normal to the faces of a crystal to which a uniaxial stress is applied , and we obtain P = d T . We see that d has only one component, T11 111 i i11 11 is the component of polarization parallel to the uniaxial stress. Thus, under these special experimental conditions, d111 is the component of polarization normal to the face of the crystal to which a uniaxial stress is applied.

Application to a crystal with point group 4mm: The non-zero components of the piezoelectric tensor are given in Table 15.2 and Equation (15.25) becomes d111 = s3 [(s21 + s22 )(d15 + d31 ) + s23 d33 ]. If we use the spherical coordinates of s (r = 1, θ, ϕ), we obtain d111 = cos θ[sin2 θ(d15 + d31 ) + cos2 θd33 ]. This longitudinal piezoelectricity coeﬃcient does not depend on azimuth ϕ. The longitudinal piezoelectricity surface is therefore a surface of revolution around the axis Ox3 , the 4-fold axis. Its section by a meridian plane is shown on Figure 15.4 for the case of barium titanate BaTiO3 in its tetragonal phase (between 120◦ C and 5◦ C). We note that for θ > π/2 the value of d111 is negative. This is why the sign − is inserted in the center of the lobe corresponding to the half-space with negative x3 .

15.3.5. Other forms of piezoelectric coeﬃcients The above piezoelectric coeﬃcients connect polarization to stress and relation (15.17b) shows that they are isothermal coeﬃcients (at constant temperature). For some applications, it is more convenient to express polarization as a function of strain, be it through isothermal or adiabatic (constant entropy) coeﬃcients. Let us focus on isothermal coeﬃcients. The thermodynamic variables must then be temperature, electric ﬁeld and strain. The thermodynamic function to consider is another Gibbs function G2 : G2 = U − ΘS − Ei Di , dG2 = −SdΘ − Di dEi + Tij dSij .

(15.26)

330

Symmetry and Physical Properties of Crystals 10–12 C/N 150 100 50

+

0 – 50

–

– 100 – 150

Figure 15.4: Intersection of the longitudinal piezoelectricity surface of a crystal of barium titanate (BaTiO3 ), with point group 4mm, by a plane passing through the 4-fold axis, which is an axis of revolution for this surface With the same approach as in Section 15.1.2 and Section 15.1.3, we obtain ΔS = (C/Θ)ΔΘ + pi Ei + λkl Skl ,

(15.27a)

Dj = pj ΔΘ + εji Ei + ejkl Skl ,

(15.27b)

Tmn = −λmn ΔΘ − eimn Ei + cmnkl Skl .

(15.27c)

Clearly the coeﬃcients pi are pyroelectric coeﬃcients at constant temperature and strain, while in Equations (15.17) they were the constant temperature and zero stress coeﬃcients. Their diﬀerence will be calculated in Section 15.4. We note that the coeﬃcients eijk appear with opposite signs. The explanation is simple, since they are obtained through: Dj = −

∂Dj ∂ 2 G2 ∂G2 from (15.26) and =− . ∂Ej ∂Skl ∂Ej ∂Skl

We set: ejkl = −

∂ 2 G2 . ∂Ej ∂Skl

On the other hand Tmn =

∂G2 ∂Smn

and

∂Tmn ∂ 2 G2 = = −eimn ∂Ei ∂Ei ∂Smnl

from deﬁnition (15.28). The opposite signs for the λij have the same origin.

(15.28)

Chapter 15 – Crystal thermodynamics. Piezoelectricity

331

In piezoelectricity problems involving constant temperature, we then use the two equations: Dj = εji Ei + ejkl Skl , Tmn = −eimn Ei + cmnkl Skl .

15.3.6. Applications Materials used Piezoelectric materials can be used under various forms: single crystal form: the best known is quartz, a natural crystal which is also manufactured, often as large single crystals with excellent quality (Fig. 1.3). Other important single crystal materials are berlinite (AlPO4 ), gallium orthophosphate (GaPO4 ), gallium arseniate (GaAsO4 ), lithium niobate (LiNbO3 ), lithium tantalate (LiTaO3 ). ceramics: if the piezoelectric material is also ferroelectric, it can be used in the form of a polarized ceramic, i.e. of a compacted and sintered powder, the grains of which are reoriented by applying a strong electric ﬁeld (see Sect. 15.2). Among the materials used in ceramic form are barium titanate (BaTiO3 ), potassium niobate (KNbO3 ), lead zirconate–titanate Pb(Zrx Ti1−x )O3 , designated as PZT. thin crystal ﬁlms polymers: some polymers such as polyvinylidene ﬂuoride (PVDF) become piezoelectric if their molecules are oriented by a mechanical or electrical process. Application areas There are many areas of application, and the list below is not exhaustive. Converting an electrical wave into an acoustical wave, i.e. production of ultrasound, and conversely conversion of an acoustic wave into an electrical signal for ultrasound reception. These two eﬀects make it possible to emit ultrasound waves and to receive those scattered by the medium. This is why they are used in medicine for echography and in sonars (the acronym for SOund Navigation And Ranging) to detect objects in water and determine their distance.6 In the range of audible frequencies, production of microphones and loudspeakers, in particular for cellular telephones. Pressure sensors: pressure on the piezoelectric material generates a measurable electrical signal. 6. The sonar was invented by Paul Langevin and Constantin Chilowski in 1917 and used during World War I.

332

Symmetry and Physical Properties of Crystals Micro-manipulators: an applied voltage generates a strain which leads to micro-displacements. Piezoelectric resonators: elastic waves propagate in a crystal as modes which depend on its shape, dimensions and nature. The piezoelectric effect, which couples the mechanical and electric quantities, makes it possible to generate these vibration modes. This produces resonators which vibrate, when an electrical signal is applied, at a perfectly deﬁned frequency, stable over long periods of time. Quartz watches thus use the resonance of a quartz tuning-fork shaped crystal to generate regular time pulses. The use of quartz crystals with special orientation, shape and dimensions make it possible to obtain resonators whose frequency practically does not vary with temperature. The resonance frequency of this type of oscillators is extremely sensitive to the mass of the crystal, yielding quartz balances capable of detecting extra masses on the order of an atomic monolayer. High voltage generation through application of a stress: this eﬀect is used in gas lighters.

15.4. Principal and crossed eﬀects under various conditions In the preceding sections (except for Sect. 15.3.5), the various tensors representing principal or crossed eﬀects connect a conjugate-type quantity to a thermodynamic coordinate-type quantity for constant values of the two conjugate quantities which do not enter the relation. For example tensor smnkl connects stress Tkl to strain Smn at constant temperature and zero or constant electric ﬁeld. Equation (15.17c) then yields: Smn = smnkl |E,Θ Tkl . and smnkl |E,Θ is the isothermal elastic coeﬃcient. The same coeﬃcient at constant entropy, ΔS = 0 and zero electric ﬁeld is denoted as smnkl |E,S and we now determine the relation connecting them. If ΔS = 0, the change in temperature is no more zero. It is given by Equation (15.17a), i.e. 0 = (C/Θ)ΔΘ + αkl Tkl

and

ΔΘ = −(Θ/C)αkl Tkl .

Equation (15.17c) becomes Smn = −αmn (Θ/C)αkl Tkl + smnkl Tkl = (−αmn (Θ/C)αkl + smnkl )Tkl or with

Smn = smnkl |E,S Tkl smnkl |E,S = smnkl |E,Θ − (Θ/C)αmn αkl .

Chapter 15 – Crystal thermodynamics. Piezoelectricity

333

Table 15.4: Order of magnitude of the principal and crossed eﬀects deﬁned in this chapter, expressed in International System (SI) units ΔΘ

Ei

Tkl

ΔS

(C/T ) 104

p 10−6

[α] 10−5

Dj

p 10−6

ε0 [ε] 10−10

[d] 10−12

Smn

[α] 10−5

[d] 10−12

[s] 10−11

Table 15.4 allows us to calculate the order of magnitude of the diﬀerence between these isothermal and adiabatic coeﬃcients, viz. 10−4 . 10−5 . 10−5 = 10−14 , while smnkl |E,Θ is on the order of 10−11 , thus larger by three orders of magnitude. The diﬀerence is negligible. This kind of calculation can be performed for all the other tensors, considered under various conditions. For example the diﬀerence between the zero electric ﬁeld and the zero induction elastic constants, with both measurements performed at constant temperature, can be calculated. Generally, the relative diﬀerence between these two coeﬃcients is much smaller than 1. This is not the case for the pyroelectric vector measured at zero stress, denoted by pi |Tkl =0 , and at zero strain, pi |Skl =0 , the electric ﬁeld being zero in either case. At zero stress and electric ﬁeld, Equation (15.17b) can be written as: Pj = pj |Tkl =0 ΔΘ. For a temperature variation ΔΘ at zero strain, Smn = 0, the stress Tkl is no more zero. It is given by Equation (15.17c): 0 = αmn ΔΘ + smnkl Tkl .

(15.29)

To obtain the value of Tkl from this equation, we use the contracted notation for Tkl and αmn in order to use the elastic coeﬃcients under the contracted form sμν , and the matrix c inverse to matrix s. Equation (15.29) can be written, for each value of β, as sβν Tν + αβ ΔΘ = 0.

(15.30)

The matrix of compliance components {sβν } is the inverse of the matrix {cλμ } of stiﬀness components, which translates into relation sβν cνμ = δβμ .

(15.31)

We multiply Equation (15.30) by cμβ , then sum the six equations, with β varying over the range 1 to 6. We obtain: cμβ sβν Tν + cμβ αβ ΔΘ = 0. Using relation (15.31), the ﬁrst term in this equation is equal to δμν Tν = Tμ , and we obtain Tμ = −cμβ αβ ΔΘ

334

Symmetry and Physical Properties of Crystals

so that Tkl = −cklmn αmn ΔΘ equivalent to (15.29). Equation (15.17b) becomes Pj = pj |Tkl =0 ΔΘ − djkl cklmn αmn ΔΘ = pj |Skl =0 ΔΘ. We obtain: pj |Skl =0 = pj |Tkl =0 − djkl cklmn αmn . The diﬀerence between the two pyroelectric eﬀects is, according to Table 15.4, on the order of 10−6 , i.e. on the same order as the pyroelectric eﬀect. This means that the pyroelectric vector at zero strain is diﬃcult to measure, because it is extremely small. It is called primary pyroelectricity, while the term djkl cklmn αmn which is to be added to obtain the pyroelectric vector at constant stress is called secondary pyroelectricity. If the crystal is not submitted to stress during the change in temperature, it is free to deform through thermal expansion. This deformation produces, through piezoelectricity, a polarization which is secondary pyroelectricity.

15.5. Exercises Exercise 15.1 Show that all the components of the piezoelectric tensor for group 432 are zero although this group is not centrosymmetric. Use the tensor form given in Table 15.2 for group 422, a subgroup of 432, and supplement it with the additional symmetry operation that leads to group 432. Exercise 15.2 Consider a crystal with point group ¯42m, assuming the form of the tensor is known for one of its subgroups, 222 or mm2. Choose the axis Ox3 parallel to the ¯4 axis. 1.

Determine the non-zero coeﬃcients of the piezoelectric tensor in the two following cases: (a) Ox1 is chosen parallel to one of the 2-fold axes, (b) Ox1 is chosen perpendicular to one of the mirrors.

2.

The compound (NH4 )H2 PO4 (ammonium dihydrogen phosphate, ADP), with point group ¯42m, has, in the axis system deﬁned in question (1a), the piezoelectric coeﬃcients: d14 = d25 = 0.17 × 10−11 C N−1 and d36 = 5.17 × 10−11 C N−1 . Determine its piezoelectric coeﬃcients in the axis system deﬁned in question (1b).

Chapter 15 – Crystal thermodynamics. Piezoelectricity

335

Exercise 15.3 Show that the longitudinal piezoelectricity surface for a crystal with point group 422 vanishes for all directions. (A similar result would be obtained for group 622). The form of the piezoelectric tensor for group 422 is given in Table 15.2. Exercise 15.4 Quartz SiO2 belong to group 32, for which the form of the piezoelectric tensor is given in Table 15.2 for the axis system where Ox3 is parallel to the 3-fold axis and Ox1 is parallel to a 2-fold axis. 1.

A uniaxial stress T is applied to a quartz crystal along a direction in the plane (Ox1 , Ox2 ). Call θ the angle between the direction of the stress and axis Ox1 . (a) Show that the obtained polarization P has a norm independent of θ. (b) How does the direction of P vary when θ varies? (c) What uniaxial stress should be applied to the crystal in order to obtain a polarization along Ox2 ?

2.

Calculate the longitudinal piezoelectric coeﬃcient for a general direction. Represent the intersection of this surface with the plane (Ox1 ,Ox2 ). Deduce the overall look of the longitudinal piezoelectric surface.

Exercise 15.5 Zinc sulﬁde ZnS is a cubic crystal with point group ¯43m. 1.

A rectangle parallelepiped with sides parallel to the vectors a, b and c of the unit cell is cut out of this crystal. What stress (or stresses) should be applied onto this parallelepiped to determine the value of d14 ?

2.

Calculate the longitudinal piezoelectric coeﬃcient in a general direction deﬁned by its direction cosines s1 , s2 , s3 . Express it as a function of the spherical coordinate angles θ and ϕ.

3.

Calculate the values of ϕ and θ for which the longitudinal piezoelectric coeﬃcient is maximum.

4.

A cube of ZnS with sides parallel to directions [110], [¯110] and [001] is submitted to a uniform electric ﬁeld E, parallel to [001]. The value of this ﬁeld is 5 × 105 V m−1 . (a) Show that the volume variation of the crystal under the eﬀect of the applied electric ﬁeld is zero. (b) Determine the relative variation in the lengths of the sides of the cube. The value of d14 is 2 × 10−11 C N−1 .

336

Symmetry and Physical Properties of Crystals

Exercise 15.6 1.

Quartz, with point group 32, is piezoelectric. We try to predict, using Curie’s principle, whether the application of a uniaxial stress along some simple crystallographic directions can lead to a polarization. Consider in turn the cases where: (a) the uniaxial stress is parallel to the 3-fold axis, (b) the uniaxial stress is parallel to a 2-fold axis, (c) the uniaxial stress is parallel to Ox2 , with Ox1 being parallel to the 2-fold axis of (b), (d) the stress is a shear T12 .

2.

Zinc oxide ZnO, with point group 6mm, is piezoelectric. We discuss the same questions as in (1), viz. whether a polarization can exist under the inﬂuence of a uniaxial stress. We choose an orthonormal axis system where Ox3 is parallel to the 6-fold axis and Ox1 is perpendicular to one of the mirrors. Consider the following cases: (a) the uniaxial stress is parallel to Ox3 , (b) the uniaxial stress is parallel to Ox1 , (c) the uniaxial stress is parallel to Ox2 . For each case, check the results by using the appropriate piezoelectric tensor, as given in Table 15.2.

Exercise 15.7 Consider a crystal with point group ¯42m. Choose an orthonormal axis system (Ox1 x2 x3 ) where Ox1 and Ox2 are parallel to the 2-fold axes. Using Curie’s principle, determine whether a shear stress T12 allows a polarization to exist. Same question if the shear stress rotates by 45◦ around axis Ox3 . Check the obtained results by using the piezoelectric tensor for group ¯42m.

Chapter 15 – Crystal thermodynamics. Piezoelectricity

337

Complement 15C. Electrostriction and magnetostriction Piezoelectricity is discussed in Section 15.3. It relates, through Sij = dijk Ek , an electric ﬁeld with the strain, linear with respect to the ﬁeld, which it produces or, conversely, it relates the stress to the electrical polarization, again with a linear dependence. It is present only in crystals belonging to some point groups, and in particular lacking a center of symmetry. Electrostriction is more general a property. It relates an electric ﬁeld with the strain it produces, but now the strain is proportional to the square of the electric ﬁeld in the case of an isotropic material, or bilinear in the ﬁeld components for an anisotropic material: Sij = Qijkl Ek El . This property, represented by a rank-4 tensor, is featured by all insulating materials (dielectrics), including liquids and crystals of any symmetry, but its intensity varies considerably. Piezomagnetism, the magnetic analogue of piezoelectricity, was long believed to be impossible, until this was shown to be wrong in the late 1950’s. It is however a weak eﬀect, and is restricted to materials with special (magnetic) symmetry, such as the antiferromagnets MnF2 , CoF2 and NiF2 . Magnetostriction is the magnetic eﬀect roughly corresponding to electrostriction. It too varies considerably among materials. Large eﬀects are encountered in ferro- or ferrimagnets, i.e. materials which have, at the microscopic level, an ordered magnetic structure. The main contribution is due to the growth, under an applied magnetic ﬁeld, of the domains7 with magnetization direction near that of the ﬁeld; at saturation, the strain is the spontaneous magnetostrictive strain, whereas the demagnetized state as well as the zero-ﬁeld state involve an average over the domain magnetization directions. The most eﬃcient magnetostrictive material is Terfenol D, a rare-earth–iron compound with formula8 Tbx Dy1−x Fe2 , with x ∼ 0.3, in which strains of the order of 2 × 10−3 are encountered. Both magnetostrictive and electrostrictive materials are important for applications, the more obvious ones being sensors and actuators. One of the advantages of the magnetic version is the fact that a magnetic ﬁeld can be applied through external coils and magnetic circuits, and does not require voltage to be applied on the actuator or sensor itself.

7. See the footnote in Complement 8C. 8. The “nol” at the end of Terfenol has nothing to do with the international organic chemistry nomenclature, which links “ol” to alcohols: it just celebrates the (U.S.) Navy’s Ordnance Laboratory, where research on magnetostrictive materials has long been very active toward the development of sonar for underwater sensing.

338

Symmetry and Physical Properties of Crystals

Further reading E. du Trémolet de Lacheisserie, D. Gignoux and M. Schlenker (ed.), Magnetism, vol. 1: Fundamentals (Springer Verlag, New York and Heidelberg, 2005), chap. 12 E. du Trémolet de Lacheisserie, D. Gignoux and M. Schlenker (ed.), Magnetism, vol. 2: Materials and Applications (Springer Verlag, New York and Heidelberg, 2005), chap. 15

Chapter 15 – Crystal thermodynamics. Piezoelectricity

339

References [1] L.D. Landau, E.M. Lifshitz and L.P. Pitaevskii, Course of Theoretical Physics, vol. 8, Electrodynamics of Continuous Media, 2nd edn. (Elsevier, Oxford, 1984) [2] H.B. Callen, Thermodynamics and an Introduction to Thermostatistics, 2nd edn. (Wiley, New York, 1985) [3] J.F. Nye, Physical Properties of Crystals: Their Representation by Tensors and Matrices (Oxford University Press, Oxford, 1985) [4] Landolt and Börnstein Tables, vol. III.2 (Springer Verlag, Berlin, 1969)

Chapter 16

Light propagation in crystals When an electromagnetic wave propagates in a crystal, the material becomes electrically polarized by the electric ﬁeld of the wave since its electrical permittivity is diﬀerent from that of vacuum. The propagation of electromagnetic waves is governed by Maxwell’s equations. In the case of anisotropic materials, these yield the birefringence of crystals, which is thoroughly discussed.

16.1. Maxwell’s equations Assuming an uncharged, non-conducting material, Maxwell’s equations have the form: div D = 0 curl E = −

E

(16.1a) ∂B ∂t

div B = 0 ∂D curl H = ∂t

(16.1b) (16.1c) (16.1d)

where D is the electrical induction deﬁned in (15.3) and again here in (16.3), the electric ﬁeld, B the magnetic induction, H the magnetic ﬁeld. Since we consider non-magnetic materials: B = μ0 H where μ0 is the magnetic permeability of vacuum (μ0 = 4π × 10−7 in SI units), hence div H = 0

(16.1e)

∂H . (16.1f) ∂t Dielectric materials polarize under the inﬂuence of an oscillating electric ﬁeld E. The polarization P is related to the electric ﬁeld by relation: curl E = −μ0

P = ε0 [χ]E © Springer Science+Business Media Dordrecht 2014 C. Malgrange et al., Symmetry and Physical Properties of Crystals, DOI 10.1007/978-94-017-8993-6_16

(16.2)

341

342

Symmetry and Physical Properties of Crystals

where [χ] is the electrical susceptibility tensor of the material, in the linear approximation which we adopt throughout this chapter. The materials for which this approximation is suﬃcient are linear materials. Induction D is then given by: D = ε0 E + P = ε0 E + ε0 [χ]E = ε0 [ε]E. (16.3) ε0 is the permittivity of vacuum (1/4πε0 = 9×109 in SI units) and [ε] = [E]+[χ] is the tensor of relative permittivity of the material, with [E] the unit tensor. This equation was already given in (15.3), in the discussion of permittivity in a static electric ﬁeld. Here the electric ﬁeld is rapidly variable, and the values of the coeﬃcients of the relative permittivity tensor [ε] can be very diﬀerent from their value for a static ﬁeld. If the material is isotropic, tensor [ε] reduces to a scalar, and the propagation equation for an electromagnetic wave is easily solved since condition (16.1a) then leads to div E = 0. The solution for anisotropic materials is more complicated, and we restrict our search to sinusoidal solutions. Also, we here consider only transparent materials, i.e. non absorbing materials, hence the components of tensor [ε] are assumed to be real.

16.2. Light propagation in an isotropic material We discuss propagation in either vacuum or an isotropic dielectric for which tensor [ε] is a scalar, noted ε. Using Maxwell’s equations, we calculate: curl curl E = −μ0

∂ ∂2D ∂2E (curl H) = −μ0 2 = −μ0 ε0 ε 2 ∂t ∂t ∂t

and we then use the identity: curl curl E = grad div E − ΔE. Since D and E are parallel (this will no more be the case in an anisotropic material), div E = 0 from (16.1a), and we obtain: ΔE − ε0 μ0 ε

∂2E = 0. ∂t2

(16.4)

This equation has solutions of the form: s · r (16.5) E = E0 f t ± v √ with v = 1/ εε0 μ0 , i.e. plane waves propagating in the direction of unit vector s at velocity ± v (see (14.6) and Fig. 14.1). t±

Setting si ∂f ∂E = ±E0 , ∂xi v ∂u

s·r = u, v ∂2E s2 ∂ 2 f = E0 i2 2 , 2 v ∂ u ∂xi

∂2E ∂2f = E0 2 2 ∂t ∂ u

Chapter 16 – Light propagation in crystals

343

and Equation (16.4) is veriﬁed if 1/v 2 = εε0 μ0 . In vacuum, ε = 1 and v = c. We ﬁnd the well-known relation ε0 μ0 c2 = 1. √ We deduce that, in a dielectric material, v = c/ ε. By deﬁnition, the optical index, or refractive index, of a material is n = c/v, and the above relations indicate that n2 = ε. We would of course have obtained the same solution for the magnetic ﬁeld, i.e. √ a plane wave propagating at velocity v = c/ ε.

16.3. Sinusoidal waves that are solutions of Maxwell’s equations Plane sinusoidal waves have the form: E = E0 cos(k · r − ωt)

E = E0 [exp i(k · r − ωt)]

or

(16.6)

where k = ks is the wave vector, ω is the angular frequency of the wave, and means “real part of”. We can write: cos(k · r − ωt) = cos[ω(t − ks · r/ω)]. Comparing with Equation (16.5), we see that the propagation velocity v, or phase velocity, is such that: ω (16.7) v= . k Furthermore, k · r = ks · r = k (Fig. 14.1) if is the distance from origin of a wave plane, counted along an axis parallel to s. The wavelength λ is such that, for a distance equal to λ, the argument of the cosine varies by 2π, hence λ = 2π/k. Note: if we had chosen, as is customary in crystallography and in X-ray diﬀraction, to express waves in the form cos 2π(k · r − νt) (Tab. 3.1), the norm of the wave vector would be equal to 1/λ. The frequency ν is equal to ω/2π. The sinusoidal behavior of vectors E and H makes the diﬀerentiations of vectors E or H with respect to time and to the coordinates very easy: ∂E = −i ω E, ∂t

div E = i k · E

and

curl E = i k × E.

(16.8)

The same relations are valid for vector H. Applying these relations to Equations (16.1a) and (16.1e), we obtain: k·D=0

and

k·H=0

(16.9)

so that vectors D and H are perpendicular to wave vector k. Furthermore, we deduce from Equations (16.1d) and (16.1f): k × H = −ωD,

(16.10a)

k × E = μ0 ωH.

(16.10b)

344

Symmetry and Physical Properties of Crystals

Vector D is perpendicular to H and to k from (16.10a), and H is perpendicular to k after (16.10b). We deduce that vectors k, D and H form a direct trirectangular trihedron, whether the material is isotropic or not (Fig. 16.1a). Furthermore, E is perpendicular to H (16.10b), and therefore lies in the plane deﬁned by D and k. In an isotropic material, the trihedron deﬁned by k, E and H is also a direct trirectangular trihedron (Fig. 16.1b). H

H

E

s k

D

u

k

E D

S

S

(a)

(b)

Figure 16.1: Relative orientations of vectors H, E, D, S and k. Vector H is perpendicular to the four other vectors. (a) Anisotropic material. (b) Isotropic material. The direction of energy propagation, hence of the light rays, is that of Poynting’s vector S, the norm of which represents the energy that propagates across unit area during unit time, i.e. the intensity of the light beam propagating in the direction of S: S=E×H so that S is perpendicular to E and H. In an anisotropic material, the direction of energy propagation is thus usually diﬀerent from that of the wave vector, and thus the propagation velocity of energy is diﬀerent from the propagation velocity of the wave planes, which is the phase velocity deﬁned in (16.7). In an isotropic material, S is parallel to k. It is then easy to calculate the norm of S, because vectors E, H and S form a trirectangular trihedron. Using relation (16.10b), we ﬁnd: S = E H = kE 2 /μ0 ω = E 2 /μ0 v = ε0 εvE 2 . In an isotropic material, and in particular in air, the intensity of an electromagnetic wave is thus proportional to the square of the norm of the electric ﬁeld.

Chapter 16 – Light propagation in crystals

345

16.4. Plane monochromatic wave in an anisotropic material 16.4.1. Basic equation In an anisotropic material, the polarization P induced by an electric ﬁeld E is, in general, no more parallel to E. It is related to E by the electrical susceptibility tensor [χ]: P = ε0 [χ]E and

D = ε0 E + P = ε0 ([E] + [χ])E = ε0 [ε]E.

(16.11)

[ε] is the relative permittivity tensor of the crystal. This tensor is symmetric (Sect. 15.1.3). Condition div D = 0 does not lead to zero divergence for E any more, and the propagation equation obtained in (16.4) is no more valid. To simplify the problem, we seek, for the electromagnetic wave, a sinusoidal solution, so that the results of Section 16.3 can be used. We saw that the trihedron D, H, k is trirectangular. Vectors E and D are no more parallel, but enclose an angle ϕ. Since E is perpendicular to H, it is in the plane deﬁned by D and k (Fig. 16.1a). Poynting’s vector is perpendicular to E and H. It is therefore also in plane (D, k) and encloses with vector k the same angle ϕ. Using Equations (16.1b) and (16.1d), we obtain: curl curl E = −μ0

∂2D . ∂t2

(16.12)

Relations (16.8) make it possible to write Equation (16.12) in the form −k × k × E = ω 2 μ0 D.

(16.13)

Furthermore, we know that any three vectors satisfy relation: A × B × C = (A · C)B − (A · B)C

(16.14)

so that Equation (16.13) becomes: −k(k · E) + k 2 E = ω 2 μ0 D. Since the propagation velocity v of the wave (the phase velocity) is such that v = ω/k (Eq. (16.7)) and since the refractive index is deﬁned by n = c/v, so that n = ck/ω and ε0 μ0 c2 = 1, we deduce that k2 /(ω 2 μ0 ) = ε0 n2 . Setting, as before, k = ks, we obtain: D = ε0 n2 [E − s(s · E)] and

2

[ε]E = n [E − s(s · E)].

(16.15a) (16.15b)

346

Symmetry and Physical Properties of Crystals

Equation (16.15b) is actually a system of three equations: [εij + n2 si sj ]Ej = n2 Ei which are linear and homogeneous equations for E1 , E2 and E3 . For such a system to have solutions, its determinant must be zero. By expressing this condition, we obtain a relation giving the value of index n as a function of the propagation direction s. Because calculating the determinant is tedious, we will use some calculational tricks which lead to the result more easily. We start from Equation (16.15a), and use the fact that D · s = 0.

16.4.2. Birefringence The second-rank, real and symmetric tensor [ε] has three mutually orthogonal principal axes (Sect. 10.2.2). In the coordinate system of these principal axes, the tensor is diagonal: ⎞ ⎛ ε1 ⎠ ⎝ ε2 ε3 and, in the same frame, the components Di and Ei of D and E respectively are related through: D1 = ε0 ε1 E1 ,

D2 = ε0 ε2 E2,

D3 = ε0 ε3 E3 .

(16.16)

Equation (16.15a), when projected onto principal axis Ox1 , yields, using (16.16):

n2 = −s1 (s · E) D1 1 − ε1 ε1 s1 or D1 = − (s · E). (16.17a) ε1 − n2 In the same way, we obtain: ε2 s2 (s · E), ε2 − n2 ε3 s3 D3 = − (s · E). ε3 − n2 D2 = −

(16.17b) (16.17c)

Multiplying (16.17a) by s1 , (16.17b) by s2 and (16.17c) by s3 , and adding them, we obtain for the left-hand side Di si = D · s = 0, hence s2 εi i = 0. εi − n2

(16.18)

i

Expanding (16.18) yields: s21 ε1 (ε2 − n2 )(ε3 − n2 ) + s22 ε2 (ε3 − n2 )(ε1 − n2 ) +s23 ε3 (ε1 − n2 )(ε2 − n2 ) = 0.

(16.19)

Chapter 16 – Light propagation in crystals

347

This equation f (n2 ) = 0 is a second-degree equation for n2 . It is easy to show that it has two solutions. We rank the values of εi in increasing order, for example ε1 < ε2 < ε3 . The value of f (n2 = ε1 ) is positive, that of f (n2 = ε2 ) is negative and that of f (n2 = ε3 ) is positive. The continuous function f (n2 ) therefore goes to zero for two values of n2 , one between ε1 and ε2 , the other between ε2 and ε3 . One value of n2 corresponds to a single value of n, because a negative index would be equivalent to a negative velocity, simply describing a wave propagating the other way. This is why only positive indices are considered. For a given propagation direction, there are thus two values of the refractive index, hence two waves can propagate: they are called the eigenmodes. The material is said to be birefringent, or one says there is birefringence. From now on, we set: n1 =

√

ε1 ,

n2 =

√

ε2 ,

n3 =

√

ε3

(16.20)

and n1 , n2 and n3 are called the principal indices (meaning the indices associated to the principal values of tensor [ε]).

16.4.3. Index surface The index surface is the locus of points M such that OM = n s, where n is the value of the index for a wave with wave-vector parallel to unit vector s.1 Since there are two values of n for one propagation direction s, the index surface intersects any radius vector at two points. Biaxial materials We saw (Sect. 10.5) that symmetric rank-2 tensors, representing physical properties of triclinic, monoclinic or orthorhombic crystals, have three principal values which normally are diﬀerent. Therefore, for such crystals, ε1 = ε2 = ε3 , and we obtain an index surface as shown on Figure 16.2a, where only oneeighth of the surface is represented because this surface is symmetrical with respect to planes s1 = 0, s2 = 0 and s3 = 0. If s1 = s2 = 0, and therefore s3 = 1, Equation (16.19) leads to n2 = ε1 √ and n2 = ε2 . The index surface intersects axis Ox3 at x3 = ε1 = n1 and √ √ x3 = ε2 = n2 . In the same way, it intersects axis Ox1 at x1 = ε2 = n2 and √ √ √ x1 = ε3 = n3 and axis Ox2 at x2 = ε3 = n3 and x2 = ε1 = n1 . It is easy to show that the intersections of the index surface by the planes xi = 0 corresponding to si = 0 consist of a circle and an ellipse. These curves do not intersect in planes x1 = 0 and x3 = 0, but they do intersect in plane x2 = 0. Because of the symmetry of the index surface, there are in this plane four points of intersection, deduced from one another by symmetries with respect 1. The index surface is also called the wave vector surface when the length along s is taken equal to kn instead of n, k being the modulus of the wave vector in vacuum.

348

Symmetry and Physical Properties of Crystals x3

x3

n2 n1

I

I

x1

n3

n3

n1

O

I’’’

x2

n2

x1

O I’

(a)

I’’

(b)

Figure 16.2: Index surface in the general case. (a) Intersection of the surface with the planes of the orthonormal trihedron formed by the principal axes of tensor [ε]. We assume ε1 < ε2 < ε3 so that n1

s21 ε1 (ε3 − n2 ) + s22 ε1 (ε3 − n2 ) + s23 ε3 (ε1 − n2 ) = 0, hence ε1 (ε3 − n2 )(s21 + s22 ) + ε3 (ε1 − n2 )s23 = 0 and ε1 ε3 − n2 ε1 (s21 + s22 ) − n2 ε3 s23 = 0.

The index surface is deﬁned as the locus of the ends of vectors r such that r = ns, hence xi = nsi . Hence the equation of the second surface is given by: ε1 (x21 + x22 ) + ε3 x23 = ε1 ε3 , or or again

x21 + x22 x23 + = 1, ε3 ε1 x21 + x22 x2 + 32 = 1. 2 ne no

Chapter 16 – Light propagation in crystals

349

This is an ellipsoid of revolution around direction Ox3 , and tangent to the ordinary sphere along axis Ox3 (Fig. 16.3). The two optical axes which were deﬁned for biaxial materials now coincide. There is a single optical axis (whence the name uniaxial crystals), parallel to the n-fold rotation axis with order n larger than 2 (which itself is parallel to basis vector c). If ne > no , the crystal is said to be uniaxial positive (Fig. 16.3a), and if ne < no it is uniaxial negative (Fig. 16.3b). x3

x3 no

no ne

ne x2

x2

(b)

(a)

Figure 16.3: Index surface of a uniaxial crystal. Axis Ox 3 is an axis of revolution. (a) Uniaxial positive crystal. (b) Uniaxial negative crystal. Cubic crystals For cubic crystals, the three principal values of tensor [ε] are equal, and these crystals are isotropic for electromagnetic wave propagation.

16.4.4. Index ellipsoid We will see in the next section that determining the induction vectors D associated to a given propagation direction involves the tensor inverse to [ε] and its associated quadric, called the index ellipsoid, which we now introduce. The relative permittivity tensor [ε] relates E to D/ε0 through: D = [ε]E. ε0

(16.21)

The inverse tensor, called the electrical impermeability tensor, relates D/ε0 to E through: D E =[η] . (16.22) ε0 In the coordinate system of the principal axes of tensor [ε], relation (16.21) takes the form: D2 = ε2 E2 , ε0

D1 = ε1 E1 , ε0 whence

D1 E1 = ε0

1 ε1

= η1

D3 = ε3 E3 , ε0

1 D1 if we set η1 = . ε0 ε1

(16.23)

350

Symmetry and Physical Properties of Crystals

In the same way, we obtain: D2 ε0 D3 = η3 ε0

E2 = η2 E3

1 , ε2 1 with η3 = . ε3 with η2 =

Thus tensors [ε] and [η], inverse to each other, have the same principal axes, and their principal values are reciprocal to each other. The equation of the representative quadric of tensor [η], in the coordinate system of its principal axes, is: η1 x21 + η2 x22 + η3 x23 = 1. The values ηi are always positive since, from (16.23) and (16.20) ηi =

1 1 = 2. εi ni

(16.24)

Hence the quadric is, in all cases, an ellipsoid, called the index ellipsoid. It can also be written as: x22 x23 x21 + + = 1. n21 n22 n23 The semi-axes along the principal axis directions of this ellipsoid are n1 , n2 and n3 . For uniaxial crystals (tetragonal, rhombohedral and hexagonal), the index ellipsoid is of revolution around the axis of order larger than 2 which is always chosen as the Ox3 axis. Earlier, we noted n1 = n2 = no and n3 = ne . The index ellipsoid then has for its equation: x2 x21 + x22 + 32 = 1. 2 no ne

(16.25)

16.4.5. Determining the induction vectors We saw that the induction vector D is perpendicular to the wave vector, hence to unit vector s. If we choose an orthonormal coordinate system (Ox1 x2 x3 ) such that Ox3 is parallel to s, vector D has only two non-zero components, D1 and D2 . They can be obtained by projecting Equation (16.15a), reproduced below, onto the plane (Ox1 x2 ) perpendicular to s. D = ε0 n2 [E − s(s · E)].

(16.15a)

The second term in the right-hand side of this equation has zero projection, and we obtain: Di = ε0 n2 Ei . Also, the projection of Equation (16.22) yields: Dj ε0 Ei = ηij

Chapter 16 – Light propagation in crystals

351

are the components of the electrical impermeability tensor in the where the ηij chosen axis system (which need not be that of the principal axes).

We obtain:

1 D, (16.26) n2 i a system of two linear and homogeneous equations with two unknowns (D1 and D2 ), which is none other than the eigenvector equation of matrix }, a second-rank matrix whose eigenvalues are the values of 1/n2 . {ηij Dj = ηij

The representative surface of tensor [η] is the index ellipsoid. In the subspace formed by Ox1 and Ox2 , the representative surface of this same tensor is the intersection of the ellipsoid by the projection plane, hence an ellipse (Fig. 16.4). Therefore the solutions for D are vectors parallel to the axes of this ellipse. The eigenvalues are the reciprocals of the squares of the half-lengths of the axes of the ellipse (Sect. 10.2.3), hence the values of n are equal to the lengths of the semiaxes of the ellipse. x3 x’3

k O D1 D2

Figure 16.4: Determination of the induction vectors D1 and D2 of a wave with wave vector k, propagating in a birefringent crystal. D1 and D2 are parallel to the axes of the ellipse along which the index ellipsoid intersects the plane normal to vector k and going through the center of the ellipsoid. The lengths of the semiaxes of the ellipse are the values of the respective indices. Conclusion: To ﬁnd the induction vectors of a wave propagating in a crystal with its wave vector parallel to unit vector s, we consider the index ellipsoid of the crystal and its intersection by a plane going through the center of the ellipsoid, and perpendicular to vector s. This intersection is an ellipse. The two waves which can propagate (the eigenmodes) have induction vectors parallel to the axes of this ellipse, and the corresponding indices are equal to the lengths of the semiaxes of the ellipse.

352

Symmetry and Physical Properties of Crystals

Using the index ellipsoid, we can retrieve the results obtained earlier about the existence of one or several optical axes. We demonstrate it for biaxial, then for uniaxial crystals. Biaxial crystals The lengths of the three semiaxes of the ellipsoid are diﬀerent. We again rank them in order of increasing value, n1 < n2 < n3 . The intersections of the ellipsoid by a plane going through the origin are ellipses, but it can be shown that two of these intersections are circles. Consider a wave vector k in the plane (Ox1 , Ox3 ), and enclosing angle β with Ox3 . We look for the ellipse along which the ellipsoid is intersected by the plane perpendicular to k going through O (Fig. 16.5). Its semiaxes are the semiaxis of the ellipsoid parallel to Ox2 , with length n2 , and the radius of the ellipse in plane (Ox1 , Ox3 ) perpendicular to k, with length n . This length n has a value between n1 and n3 , and therefore there is an angle β for which this length is equal to n2 . The ellipse is then a circle, and wave propagation is isotropic. Let k1 be the wave vector thus deﬁned. It is clear, from the symmetry with respect to plane (Ox1 , Ox2 ), that the wave vector k2 , with angle β2 = π − β, also corresponds to a circular section of the ellipsoid. We retrieve the existence of two optical axes and their geometry in the plane perpendicular to Ox2 (Fig. 16.2b). x3 n3 k

n1 x1

O n2 x2

n’

Figure 16.5: Intersection of the index ellipsoid by its planes of symmetry. A wave with wave vector k in plane (Ox 1 , Ox 3 ) has as its indices n2 and n such that n1

Chapter 16 – Light propagation in crystals

353

x3 ne

k

x1

Do no

O

De

n no

x2

Figure 16.6: Determination of the induction vectors of a wave with wave vector k in the case of uniaxial crystals. Axis Ox 3 is parallel to the optical axis and Ox 1 perpendicular to the plane (k, Ox 3 ). We conclude: for uniaxial crystals, the ordinary vibration Do is perpendicular to the optic axis. The extraordinary vibration De is in the plane formed by wave vector k and the optic axis.

16.4.6. Direction of energy propagation The aim of this section is to show that Poynting’s vector is normal to the index surface. We write relations (16.10a) and (16.10b) so that they explicitly show only vectors E and H. k × E = ωμ0 H

(16.27)

k × H = −ωε0 [ε]E.

(16.28)

Consider a variation dk in the wave vector. If the variation is general, it entails not only variations dE and dH, but also dω (dω is zero only if dk is tangent to the index surface). Diﬀerentiating (16.27) and (16.28), we obtain: dk × E + k × dE = ωμ0 dH + μo Hdω,

(16.29)

dk × H + k × dH = −ωε0 [ε]dE − ε0 [ε]Edω.

(16.30)

We dot-multiply (16.29) with H and (16.30) with E after replacing E · [ε]dE by [ε]E · dE, since Ei εij dEj = εji Ei dEj because εij = εji . (H, dk, E) + (H, k, dE) = ωμ0 H · dH + μ0 H 2 dω −(H, dk, E) + (E, k, dH) = −ωε0 [ε]E · dE − E · Ddω. Subtracting both sides of these two equations : 2dk · (E × H) + dE · (H × k − ωε0 [ε]E) −dH · (E × k + ωμ0 H) =(μ0 H 2 + E · D)dω.

(16.31)

354

Symmetry and Physical Properties of Crystals

The second and third terms are zero because of (16.28) and (16.27) respectively, and Equation (16.31) becomes: 2dk · (E × H) = (μ0 H 2 + E · D)dω = 2udω if we note u the electromagnetic energy per unit volume (Born and Wolf, 1980) u=

1 1 (E · D) + (H · B). 2 2

Since we assume the material to be non-magnetic, B = μ0 H. Using the relation that deﬁnes Poynting’s vector, given in Section 16.3, S = E × H, we obtain dk · S = udω. Since S = uvS where vS is the energy propagation velocity, we deduce: vS · dk = dω. The index surface is the constant ω surface in wave vector space. Therefore, if dk has any value in the plane tangent to the index surface, we have dω = 0 and vS is perpendicular to dk. Hence the ray direction, which is the direction of energy propagation vS , is perpendicular to the index surface. We note that E, being perpendicular to vS , is tangent to the index surface.2

16.5. Refraction of a plane wave at the boundary between two materials 16.5.1. The wave-vectors follow the Snell-Descartes law Boundary between two isotropic materials When a wave which propagates in an isotropic ﬁrst material (1) reaches the boundary with a second isotropic material (2), it splits into two waves: one, the refracted wave, propagates in material (2), the other one is reﬂected into material (1). Let E1 , k1 be the electric ﬁeld and the wave vector of the incident wave, E2 and k2 those of the refracted wave, E3 and k3 those of the reﬂected wave. We have:

E1 = E01 exp i(k1 · r − ωt), E2 = E02 exp i(k2 · r − ωt), E3 = E03 exp i(k3 · r − ωt).

The boundary condition on the electric ﬁeld must be satisﬁed at all points on the separation surface and at all times, which implies that the space (and time) 2. The energy propagation velocity, i.e. the group velocity, can be written in the form vS = ∂ω/∂k, a condensed notation for vS1 = ∂ω/∂k1 etc. This is the generalization of the familiar expression for the group velocity in an isotropic material, ∂ω/∂k.

Chapter 16 – Light propagation in crystals

355

variations must be the same. We choose an orthonormal axis system Oxyz so that the origin O is on the separation surface and Oz is perpendicular to this surface. At any point on the surface z = 0, we must therefore have: k1x x + k1y y = k2x x + k2y y = k3x x + k3y y. These equalities must hold whatever the values of x and y. This implies that k1x = k2x = k3x

and

k1y = k2y = k3y .

Thus the tangential component of the wave vector is conserved in refraction and reﬂection. Furthermore, in the isotropic materials we are considering in this section, the rays are parallel to the wave-vectors. This property leads to the Snell-Descartes laws, which have the following expression: 1.

The refracted ray and the reﬂected ray are in the plane of incidence, deﬁned as the plane containing the incident wave vector and the normal to the interface.

2.

The reﬂection angle i3 is equal to the incidence angle i1 . The refraction angle i2 and the incidence angle i1 are related by: n1 sin i1 = n2 sin i2 .

(16.32)

The derivation of these results is straightforward if we look at Figure 16.7a. z

z M3

k1

i1 i3

k3 H material 1 material 2

O i2

i1 i2

k2

M1

M1 M2

M2 (a)

n2

k1

k1

k2

n1

H O

(b)

Figure 16.7: A wave with wave-vector k1 in an isotropic medium 1 gives rise to a reﬂected wave and a refracted wave. (a) Showing the continuity of the tangential component of the wave-vectors at the interface. (b) Construction of the refracted wave-vector k2 when medium 2 is isotropic.

356

Symmetry and Physical Properties of Crystals

The tangential component OH of the incident wave-vector k1 = OM1 is equal to the tangential components of the reﬂected wave-vector k3 = OM3 and of the refracted wave-vector k2 = OM2 . Therefore, vectors k3 and k2 are in the plane of incidence. If n1 and n2 are the indices of materials 1 and 2 respectively, k1 = k3 = k0 n1

and

k2 = k0 n2

where k0 = ω/c is the norm of the wave-vector in vacuum. Also OH = k1 sin i1 = k3 sin i3 = k2 sin i2 . Hence

(16.33)

i1 = i3 , n1 sin i1 = n2 sin i2 .

The above properties make it easy to draw the refracted wave-vector k2 associated to a given incident wave-vector k1 . We draw, starting from point O located on the surface, the vector k1 = OM1 , giving it length n1 (which is equivalent to using k0 as the unit). In medium 2, we draw a half-circle with radius n2 , centered at O. The normal to the interface going through M1 intersects the half-circle with radius n2 at M2 , the end of vector k2 = OM2 . In the following, we will focus solely on the refracted waves. Interface between an isotropic material and an anisotropic material The incident wave, with electric ﬁeld E, gives rise to a reﬂected wave which we ignore, and to two refracted waves, with wave-vectors k2 and k2 , with electric ﬁelds E2 and E2 . This is double refraction. E1 = E01 exp i(k1 · r − ωt), E2 = E02 exp i(k2 · r − ωt), E2 = E02 exp i(k2 · r − ωt). The same argument as above shows that the tangential components of the wave-vectors are continuous at the interface between the two materials, and this leads to the Snell-Descartes laws for the wave-vectors. This is valid for the wave-vectors only, as, in a crystal, the rays are not necessarily parallel to the wave-vectors. The refracted wave-vectors are determined using the same construction as above. As in Figure 16.8, we draw from a point O of the interface, chosen as origin, the incident wave-vector k1 = OM1 , giving it length n1 , i.e. taking as the unit the wave-vector in vacuum k0 . We then draw the two sheets S and S of the index surface, centered at O. The normal to the interface drawn from M1 intersects the index surface at two points M2 and M2 , the ends of wave-vectors k2 and k2 . We thus obtain: n1 sin i1 = n2 sin i2 = n2 sin i2

Chapter 16 – Light propagation in crystals

357

z

k1 i1 O i’2

material 1 crystal

H n1 k1 i2 k2 k’2

M1 S M2

S’

M’2

Figure 16.8: Construction of the wave-vectors of waves which can propagate in a birefringent crystal when the incident wave has wave-vector k1 . S and S are the two sheets of the index surface in the crystal. where angles i1 , i2 and i2 are the incidence angle and the refraction angles for the wave-vectors. If material (1) were anisotropic, the same argument would apply to each of the wave-vectors in material (1), and each wave could give rise to two waves.

16.5.2. Application to uniaxial materials The most frequent applications of crystal birefringence involve uniaxial crystals, for which the index surface consists of a sphere and an ellipsoid of revolution around the optic axis (parallel to the 3-, 4- or 6-fold axis of the crystal). The sphere and the ellipsoid are tangent to each other at their intersection with the optical axis (Fig. 16.3). Several examples will be discussed as a function of the relative orientations of the plane of incidence and the optic axis of the crystal. We assume, for simplicity, that material 1 is isotropic, with index n1 , which makes it easy to draw the index surface related to the incident wave-vector, while retaining the full generality of the argument. We take as the unit for the wave-vectors the value k0 of the wave-vector in vacuum. We recall that the plane of incidence is the plane containing the incident wavevector and the normal to the interface. We deﬁne the principal section plane as the plane containing the optic axis and the normal to the entrance face of the crystal, i.e. the interface between the crystal and material 1, through which light enters the crystal. (a) The optic axis is perpendicular to the plane of incidence The index surface then intersects the plane of incidence along two concentric circles, with radii no and ne (Fig. 16.9a). We obtain two diﬀerent wave-vectors in the crystal. Since the rays are parallel to the normal to

358

Symmetry and Physical Properties of Crystals the index surface, the rays are, in this special case, parallel to the wavevectors. The directions of the corresponding induction vectors are obtained by recalling (see Sect. 16.4.5) that, in a uniaxial material, the ordinary vibration is perpendicular to the optic axis.

(b) The optic axis is parallel to the plane of incidence and to the entrance face The plane of incidence intersects the index surface along a circle for the ordinary surface, and an ellipse for the extraordinary surface (Fig. 16.9b). There are two distinct wave-vectors in the crystal: k2 = OM2 = ko for the ordinary ray, and k2 = OM2 = ke for the extraordinary ray. The ordinary ray is parallel to the ordinary wave-vector, while the extraordinary ray is parallel not to the extraordinary wave-vector but to the normal to the index surface at M2 (vector u on Fig. 16.9b). (c) The optic axis is parallel to the plane of incidence and at any angle to the entrance face This case is represented on Figure 16.9c. The ordinary ray is parallel to the ordinary wave-vector. The extraordinary ray is parallel to the normal at M2 to the index surface (vector u on the ﬁgure). In case (a), the principal section plane is perpendicular to the plane of incidence, while it is parallel to it in cases (b) and (c). In the most general case, the plane of incidence and the principal section plane enclose any angle. This situation is more diﬃcult to represent, because the extraordinary ray is no more in the plane of incidence.

16.6. Conclusion We showed, in this chapter, that crystals which are anisotropic with respect to light propagation (i.e. all crystals except for cubic crystals) are birefringent: an incident plane wave, with given wave-vector, gives rise in the crystal to two waves propagating with two diﬀerent indices and diﬀerent wave-vectors. For each wave, the induction vector D is perpendicular to the wave-vector. At the interface between two materials, the tangential component of the wavevector is conserved, hence a simple construction provides, for a given incident wave, the direction of the wave-vectors in the crystal. The corresponding rays are in general not parallel to the wave-vectors, but they are normal to the index surface. Most applications use uniaxial birefringent crystals (tetragonal or rhombohedral or hexagonal). The index surface then consists of a sphere and an ellipsoid of revolution, tangent to each other at their intersection with the optical axis. The induction vector Do of the ordinary wave is perpendicular to the optic axis and the induction vector De of the extraordinary wave is in the plane containing the extraordinary wave-vector and the optical axis.

Chapter 16 – Light propagation in crystals

359

z

z n1 no ne

optic axis

optic axis

n1

O

no

O M1

ne no

M’2

Re

M1 M’2 u M2

De

M2

Ro

Ee De

(a)

Re

Ro

(b) z

n1 O

ne no

opti

c ax

is

M1 M’2 u M2

Ee De Re

Ro

(c)

Figure 16.9: Construction of the refracted rays for a birefringent uniaxial crystal, using the index surface. The incident wave-vector is k1 = OM1 and the refracted wave-vectors are ko = k2 = OM2 for the ordinary wave, and ke = k2 = OM2 for the extraordinary wave. Vectors Do and Eo are always parallel. (a) The plane of incidence is perpendicular to the optic axis. Vectors De and Ee are parallel. (b) The plane of incidence is parallel to the optic axis and the optic axis is in the plane of the surface. (c) The plane of incidence is parallel to the optic axis, which encloses a non-zero angle with the surface of the crystal. In cases (b) and (c), we note that the extraordinary ray Re is parallel to the normal to the index surface at point M2 , and that De is perpendicular to wave-vector ke (while Ee is perpendicular to the ray Re ).

360

Symmetry and Physical Properties of Crystals

In this chapter, we assumed the permittivity of crystals to be real, which means that the crystals are not absorbing. This assumption of perfectly transparent crystals will be retained in all what follows. We make an exception for Figure 16.10, which shows a commonplace evidence of the anisotropic optical properties of zinc crystals, which are often large and conspicuous on zinc-plated metal surfaces, such as lamp poles or sign posts. The very fact that the crystals are visible with the naked eye is due to the dependence of the reﬂectivity on the crystal orientation of the surface.

Figure 16.10: A lamp pole surface, where the crystals comprising the zinc plating are conspicuous because of the anisotropic reﬂectivity of uniaxial zinc. The ribbon in the lower half is a centimeter scale. The contents of this chapter make it possible to solve all problems dealing with light propagation in anisotropic crystals. We therefore thought it unnecessary to make the presentation more cumbersome by adding another approach, which uses the wave surface and the appropriate geometrical construction. This alternative presentation is given in Appendix 16A for the sake of those readers who are used to this approach for isotropic materials and would prefer to use it for anisotropic crystals too.

16.7. Exercises Throughout the exercises for this chapter, the prisms are assumed to be right prisms having a right triangle with apical angle θ for their basis. For simplicity, they are called prisms with angle θ. The ﬁgures show the plane of incidence, which is always perpendicular to the lateral edges of the prism. Exercise 16.1 Calculate the maximum value of the angle δ between the direction of the wave-vector and that of the associated ray in a uniaxial crystal with indices no and ne . Find the numerical value for quartz, with no = 1.544 and ne = 1.553.

Chapter 16 – Light propagation in crystals

361

Exercise 16.2 Consider a parallel-faced slab of calcite (a uniaxial negative crystal, meaning ne < no ), cut so that the optic axis is at 45◦ to the normal to the plate. The ﬁgure below shows the principal section plane of the plate, i.e. the plane containing the normal to the plate and the optic axis. The plate is illuminated by a beam of natural light, monochromatic and perpendicular to the plane of the plate.

45°

1.

Draw the path of the light rays in the plate and after the plate. Indicate their polarization state.

2.

Calculate the deviation Δ between the ordinary and extraordinary rays emerging from the plate, if the thickness e of the plate is 1 cm and the ordinary and extraordinary indices of calcite are respectively 1.6584 and 1.4865.

Exercise 16.3 A transparent uniaxial crystal is cut into a prism with apical angle θ = 30◦ (see ﬁgure below). The optic axis is parallel to the face containing AB and perpendicular to the lateral edge of the prism. A 30°

B

1.

C

This prism is placed on a goniometer so that the entrance face for the beam is the face containing AB, and that this face is perpendicular to the incident beam. Draw the propagation directions of the beams in the prism

362

Symmetry and Physical Properties of Crystals and at the exit of the prism. The deviation δo by the prism for the ordinary beam is 26.02◦ , and the deviation δe of the extraordinary beam is 18.01◦ . Find the values of no and ne .

2.

The prism is rotated around an axis parallel to its lateral side so that the entrance face is the one containing AC, and that it is normal to the incident beam. Draw the ray paths in the prism. Calculate the numerical values of the angular deviations produced by the prism for the ordinary and extraordinary rays.

Exercise 16.4 A Glan-Foucault polarizer consists of two identical prisms with angle θ, with their optic axes parallel to the lateral edges. The prisms are separated by a thin air layer (see the ﬁgure below, where the thickness of this layer is exaggerated). 9

9

The prisms are made of calcite (no = 1.658 and ne = 1.486). The device is illuminated by a monochromatic, unpolarized beam perpendicular to the entrance face. Calculate the range of angles θ such that there is only one beam at the exit of the device. Draw the ray paths in this case, and determine the polarization of the outgoing beam. Exercise 16.5 A calcite prism ABC, with lateral sides parallel to the optic axis, is associated, as shown on the ﬁgure below, with a prism ACD made of glass with index n. The device is illuminated at normal incidence by a monochromatic beam. A

D glass 30°

30° B

9

calcite C

Chapter 16 – Light propagation in crystals

363

1.

Draw the beam paths inside the two-prism system. Indicate the polarization state of each of the two waves at the exit of the two prisms.

2.

Calculate the angle α between the two outgoing beams in the case of calcite, where no = 1.6584 and ne = 1.4865 assuming the glass has index n = 1.55.

Exercise 16.6 A Rochon prism consists of two calcite prisms (ABC and ACD on the ﬁgure below), with angle 30◦ , placed at optical contact so that they form one composite parallel-faced slab. In prism ABC, the optic axis is perpendicular to the entrance face AB. In the second prism, the optic axis is parallel to the lateral edges. The device is illuminated at normal incidence by a monochromatic beam. A

9

D

30°

30° B

C

1.

Draw the ray paths through the two-prism system. Indicate the polarization state for each of the two waves at the exit of the two prisms.

2.

Calculate the angle α between the two outgoing beams in the case of calcite, for which no = 1.6584 and ne = 1.4865.

364

Symmetry and Physical Properties of Crystals

Appendix 16A. Wave surface (or ray surface) and Huygens’ construction 16A.1. Wave surface (or ray surface) It is deﬁned by considering a point source of electromagnetic wave at O. The wave surface is the locus of the points reached by the wave after a given time t, i.e. the equal-phase surface. It is thus the locus of points M such that OM = vS u where vS is the propagation velocity of energy in the direction of unit vector u, parallel to the Poynting vector S. We ﬁrst search for the relation between the phase velocity v of the wave with wave-vector k in the crystal and the energy propagation velocity vS for the same wave. A wave plane P (Fig. 16A.1) moves perpendicular to the wavevector at velocity v, the phase velocity. After a second, it is at P , a distance v from P. During the same time interval, energy propagates from A to B along the direction of the Poynting vector S, with unit vector u. Distance AB is therefore equal to vS . Let ϕ be the angle between vectors k and S. We see that vS =

v . cos ϕ

P

(16A.1)

P’ S u vs

A

s

v k

B H

Figure 16A.1: Propagation of a wave plane from P to P over a time interval of one second. The wave-vector k is normal to P and P . We show that the wave surface can be easily deduced from the index surface because the equation describing the wave surface has a form similar to the equation yielding the index surface. Consider Equation (16.10a) which we reproduce below, and cross-multiply both of its sides with u, using for the left-hand side relation (16.14) for the double cross product: k × H = −ωD u × k × H = k(u · H) − H(u · k) = −H(u · k) because u is perpendicular to H. We deduce that: 1 k 1 1 u × D = − (u × k × H) = (u · k)H = (u · s)H = cos ϕH ω ω ω v

(16.10a)

Chapter 16 – Light propagation in crystals

365

and, using (16A.1), u×D=

1 H vS

and

H = vS (u × D).

(16A.2)

The same process is applied to Equation (16.10b): k × E = μ0 ωH

(16.10b)

u × k × E = k(u · E) − E(u · k) = −kE(u · s) because u is perpendicular to E. u×H = and

k cos ϕ 1 1 E (u × k × E) = − (u · s)E = − E=− μ0 ω μ0 ω μ0 v μ0 vS (16A.3) E = − μ0 vS (u × H).

Using (16A.3), then (16A.2), we obtain: E = −μ0 vS2 (u × u × D) = −μ0 vS2 [u(u · D) − D] so that

E = μ0 vS2 [D − u(u · D)]

(16A.4)

which can be compared to Equation (16.15a), which we repeat: D = ε0 n2 [E − s(s · E)].

(16A.5)

These two equations have the same form. This is even more conspicuous if we rewrite them in order to show E and D/ε0 instead of E and D:

v2 D D (16A.6) E = S2 −u u· c ε0 ε0 and

D = n2 [E − s(s · E)]. ε0

(16A.7)

Equation (16A.7) relates D/ε0 to E by introducing the index n for the wave with wave-vector k parallel to unit vector s and perpendicular to D. The surface n = f (s) is the index surface. On the other hand, D/ε0 and E are related by the permittivity tensor [ε]. Equation (16A.6) relates E to D/ε0 by introducing the propagation velocity of energy vS /c (i.e. this velocity expressed in units of c, the velocity of light in vacuum) in the direction of Poynting’s vector S, parallel to unit vector u and perpendicular to E. The surface v S /c = f (u) is the wave surface. On the other hand E and D/ε0 are related through the impermeability tensor [η]. Thus Equation (16A.6) deduces from (16A.7), which was used throughout this chapter, by replacing D/ε0 by E, E by D/ε0 , s by u and n by vS /c. Although they do not appear directly in the equations, it is clear that tensor [ε] is replaced by [η].

366

Symmetry and Physical Properties of Crystals

This correspondence makes it possible to deduce the equation of the wave surface from that of the index surface, given in (16.18) and expanded in (16.19): i

and

u21 η1

v2 η2 − S2 c

u2i ηi =0 v2 ηi − S2 c

vS2 2 η3 − 2 + u2 η2 η3 − c

vS2 2 + u3 η3 η1 − 2 η2 − c

vS2 vS2 η1 − 2 c2 c 2 vS = 0. c2

Since ηi = 1/εi , the wave surface has the same characteristics as the index surface provided ni is replaced by 1/ni , if the quantity represented is vS /c (or provided ni is replaced by c/ni if the quantity represented is vS ). We thus obtain, for uniaxial crystals, a wave surface consisting of two sheets: a sphere with radius 1/no (the ordinary wave surface), and an ellipsoid (the extraordinary wave surface), with equation: x21 + x22 x23 + =1 η3 η1 or

x2 x21 + x22 + 3 =1 1 1 n2e n2o

if the axis of order larger than 2 (the optic axis) is chosen as Ox3 . This is an ellipsoid of revolution around Ox3 , tangent to the ordinary sphere (Fig. 16A.2). We showed that the normal to the index surface is parallel to Poynting’s vector with unit vector u. In the same way, the normal to the wave surface is parallel to unit vector s, hence to the wave-vector k, and the induction vector D is then tangent to the wave surface. Figure 16A.2 shows the wave surface for a uniaxial material, positive in (a), negative in (b). x3

x3

1/no

1/no 1/ne

1/ne x2

(a)

x2

(b)

Figure 16A.2: Wave surfaces for uniaxial materials when the represented quantity is v S /c: (a) Uniaxial positive; (b) Uniaxial negative

Chapter 16 – Light propagation in crystals

367

16A.2. Huygens’ construction It rests on the Huygens principle, which can be expressed on the basis of envelope waves. Consider a wave surface Σ1 in a given material. One second later, this wave surface has become surface Σ2 , which is the envelope of the wave surfaces emitted by each point of Σ1 . This result applies easily to the transmission of a plane wave from one isotropic material with index n to an anisotropic material. We recall that a wave plane is a wave surface for a point emitter located at inﬁnity. Let AO be the incident ray direction in the isotropic material, and P the wave plane. Let Δ be the line along which the incident wave plane intersects the interface, one second after it went through O. The distance from Δ to plane P is equal to c/n if the isotropic material has index n. The wave plane in the crystal one second after it passed through O goes through line Δ and is tangent to the wave surface emitted at O (Fig. 16A.3). We thus obtain two wave planes, tangent respectively at M and M to the two sheets Σ and Σ of the wave surface. The rays propagate in the crystal along OM and OM . In a completely general case, points M and M are not in the plane of incidence represented on the ﬁgure. A

P c/n

O ’

M’ M

’

R’

R

Figure 16A.3: Use of the wave surface to represent the transmission of a plane wave from an isotropic material into an anisotropic material (Huygens’ construction). We draw the wave planes Π and Π going through line Δ and tangent to the two sheets of the surface. Let M and M be the contact points. The rays are given by directions OM and OM whereas the wave-vectors are perpendicular to the wave planes.

Figure 16A.4 shows the application of this method in two special cases of uniaxial materials. In (a), the optic axis is parallel to the surface and to the plane of incidence. In (b), it has a general direction but the incident ray is perpendicular to the surface.

368

Symmetry and Physical Properties of Crystals P 1/n

optic axis

1/no 1/n O

’

M’ Ee De

op tic

M

’

P

Ro Re

(a)

Ee De

1/no is

ax

Ro Re

(b)

Figure 16A.4: Use of Huygens’ construction to represent the transmission of a plane wave from an isotropic material with index n to an anisotropic uniaxial material (indices no and ne ) in the case when the optic axis is in the plane of incidence. The speed unit is here c as in Figure 16A.2. Ro and Re are the ray directions for ordinary and extraordinary rays, respectively. (a) The optic axis is in the plane of the interface. (b) The optic axis is not in the plane of the interface, and the incident ray is perpendicular to the interface. Line Δ is then at inﬁnity.

Chapter 17

Polarization of light by crystals In this chapter, we show how crystal birefringence can be used to change the polarization of an electromagnetic wave and thus obtain light in a well-deﬁned polarization state. Various devices using this birefringence are described: linear polarizers and phase shifting plates.

17.1. Polarization state of an electromagnetic wave We ﬁrst deﬁne the polarization state for a plane and monochromatic electromagnetic wave propagating in vacuum. We consider the electric ﬁeld vector rather than the magnetic ﬁeld vector because the interaction of this wave with a material, assumed here to be non magnetic (Sect. 16.1), occurs mainly through the electric ﬁeld. The electric ﬁeld of the plane wave in vacuum is perpendicular to the wave-vector. Therefore, if we choose a coordinate system where Oz is parallel to the propagation direction, the electric ﬁeld has only two components, Ex and Ey : Ex = E1 cos(kz − ωt + α)

(17.1)

Ey = E2 cos(kz − ωt + β)

(17.2)

The values of α and β depend on the origins of z and t chosen. Through an appropriate change in either of these origins, we can always obtain: Ex = E1 cos(kz − ωt) Ey = E2 cos(kz − ωt + ϕ)

(17.3) where

ϕ = β − α.

(17.4)

Because the wave is plane, it is suﬃcient to represent the electric ﬁeld E along the propagation direction, Oz. Various cases will be investigated as a function of the value of ϕ.

© Springer Science+Business Media Dordrecht 2014 C. Malgrange et al., Symmetry and Physical Properties of Crystals, DOI 10.1007/978-94-017-8993-6_17

369

370

Symmetry and Physical Properties of Crystals

17.1.1. Linearly polarized wave Assume ϕ = 0 or π. Vector E remains parallel to itself, and encloses with axis Ox an angle θ such that tan θ = E2 /E1 if ϕ = 0, and tan θ = −E2 /E1 if ϕ = π (Fig. 17.1). The polarization is called linear or rectilinear. At a given point on axis Oz, the end of vector E oscillates sinusoidally around O. y E2 =0

O

E1

x

= – E2

Figure 17.1: Linear polarizations obtained when the phase shift ϕ between the two perpendicular components is equal to 0 or to π

17.1.2. Circularly polarized wave Assume ϕ = ±π/2 and E1 = E2 : Ex =

E1 cos(kz − ωt) =

E1 cos ψ

Ey = ∓ E1 sin(kz − ωt) = ∓ E1 sin ψ if we set ψ = kz − ωt. The projection m onto a plane perpendicular to Oz of the end M of the electric ﬁeld vector describes a circle with radius E1 since Ex2 + Ey2 = E12 . At a given time t, ψ varies linearly with z and the end of the electric ﬁeld vector describes a helix with axis Oz. If we consider the upper sign (corresponding to ϕ = π/2), the helix is left-handed and we will say that the polarization is left-circular. If ϕ = −π/2, the helix is right-handed1 and the polarization is right-circular (Fig. 17.2). We note that a right-handed helix is transformed into a left-handed helix by a mirror. At a given point of the propagation axis Oz (z ﬁxed), the end of E describes, in the course of time, a circle. Consider, for simplicity, the situation at z = 0.

1. The screws used in mechanical applications are, except for highly exceptional cases, right-handed helices. The same applies to cork-screws. These right-handed screws and cork-screws penetrate into the material if they are rotated clockwise (“to the right”) as seen by an operator facing the material.

Chapter 17 – Polarization of light by crystals

Right-handed helix

371

Left-handed helix

(a) y M

x

O

z

(b)

Figure 17.2: (a) Representation of a right-handed helix and a left-handed helix for which the envelope is materialized by the generators of a cylinder; (b) representation of the variation, along the propagation direction Oz, of the electric ﬁeld vector of a right-circular wave at a given time. The locus of the ends of these vectors is a right-handed helix. Right-circular polarization (ϕ = −π/2 and the lower sign for Ey ) yields: Ex = E1 cos ωt Ey = −E1 sin ωt. Thus, an observer located at a point with z > 0 (downstream along the propagation direction, hence looking at the source) sees the polarization vector OM rotating clockwise (Fig. 17.3a). Conversely, for left circular polarization, the same observer sees the polarization vector OM rotating counterclockwise (Fig. 17.3b). y

y

M t O

t

x

O

x

M

(a) Right circular

(b) Left circular

Figure 17.3: Representation as a function of time of the end M of the electric ﬁeld vector at a given point for a right (a) and a left (b) circular wave. Axis Oz points in the propagation direction.

372

Symmetry and Physical Properties of Crystals

17.1.3. Elliptically polarized wave Consider the most general case, where E1 , E2 and ϕ have any values. We obtain the curve described by m, the projection of the end M of the electric ﬁeld vector on the plane xOy, if we eliminate (kz − ωt) between Equations (17.3) and (17.4). We obtain: Ex2 Ey2 2Ex Ey cos ϕ + − = sin2 ϕ. E1 E2 E12 E22

(17.5)

This is an ellipse, the axes of which are Ox and Oy if cos ϕ = 0, hence for ϕ = ±π/2. For other values of ϕ, it is easily shown that the axes of the ellipse enclose with axes Ox and Oy respectively the angle θ such that: tan 2θ =

2E1 E2 cos ϕ . E12 − E22

If E1 = E2 , θ equals ±π/4 for all values of ϕ. Figure 17.4 shows the trajectory described by the end of the electric ﬁeld vector at a given point as a function of time, for various values of ϕ.

=0

0 < < /2

= /2

/2 < <

=

=

< < 3/2

= 3/2

3/2 < <

= 2

Figure 17.4: Curves described by the end of the electric ﬁeld vector of a plane wave, at a given point, as a function of time, for various values of the phase shift ϕ between the two orthogonal components. The propagation direction points toward the observer. Note: if we consider an electromagnetic wave in a birefringent crystal, the vector perpendicular to the wave-vector which characterizes the polarization state is the induction vector, and all the above results apply to the components Dx and Dy of induction.

17.1.4. Natural light Classical light sources are made up of atoms oriented in all directions, with each of them emitting polarized light. The waves emitted by the various atoms are mutually incoherent. This is called “natural light” or “unpolarized light”. This light is represented as the sum of two incoherent waves, each of them linearly polarized, with their polarizations in any two perpendicular directions. Usually, light is not completely unpolarized: it is partly polarized.

Chapter 17 – Polarization of light by crystals

373

The polarization state is then conveniently described by the Stokes parameters which are deﬁned in Section 17.5. Here we consider totally polarized light, deﬁned by its two orthogonal components, and sometimes totally unpolarized natural light.

17.2. Jones notation Equations (17.3) and (17.4) can also be written as: Ex = E1 [exp i(kz − ωt)] = [E1 exp i(kz − ωt)] Ey = E2 [exp i(kz − ωt + ϕ)] = [E2 exp iϕ exp i(kz − ωt)] where means “real part of”. The type of polarization depends on the values of E1 , E2 and ϕ. The polarization of the wave is thus perfectly determined by the complex components: Ex = E1 Ey = E2 exp iϕ where ϕ is the phase shift between Ex and Ey . In what follows, we will use this complex notation, called the Jones notation, invented by R. Clark Jones in 1941. The Jones vector of the previous ﬁeld is then:

E1 . E2 exp iϕ The amplitude of the electric ﬁeld is equal to the modulus of this complex vector. If needed, the exact form of the wave is obtained by multiplying these complex components by exp i(kz − ωt) and by taking their real parts. A few examples of Jones vectors are given below, with a and b real numbers:

a . Linear polarization: b The angle θ between the electric ﬁeld and axis Ox is such that tan θ = b/a.

a Right circular polarization: . −ia

a Left circular polarization: . ia These Jones vectors for right circular and left circular polarization would have to be interchanged if the waves were described in the form exp i(ωt − kz). In contrast, the rule given by Figure 17.3 to determine whether the polarization is right-handed or left-handed remains valid whatever the choice made for describing the wave.

374

Symmetry and Physical Properties of Crystals

General polarization:

a b exp iϕ

.

17.3. Linear polarizers A linear polarizer changes any incident light into a linearly polarized light, by acting diﬀerently upon the two orthogonal directions of linear polarization. One category of linear polarizers consists of materials which absorb much more eﬃciently one polarization direction than the perpendicular direction. This is, for example, the case of Polaroid® sheets, consisting of long polymer molecules, oriented by the application of a uniaxial stress and maintained in this orientation by enclosing the polymer in a more rigid plastic foil coating. These special molecules absorb the polarization which is parallel to their long side, and transmit the polarization which is perpendicular. The other category splits the incident light into two beams with mutually orthogonal linear polarizations, retaining only one of the beams. One method is based on reﬂection at Brewster’s angle. If light with any polarization state falls under this incidence angle iB on a material with index n, glass for example, the component polarized parallel to the plane of incidence is not reﬂected. The other component, polarized perpendicular to the plane of incidence, is reﬂected, but only partly because part of the incident intensity is transmitted. This Brewster angle is such that tan iB = n. The other, more eﬃcient method, uses the birefringence properties of crystals. There are two types of such birefringent devices. The ﬁrst type uses total reﬂection of one of the two beams (ordinary (o) or extraordinary (e)) on the exit face of a prism, and thus allows only one of the two linearly polarized beams to go through. In order for the outgoing beam not to be deviated, two prisms are mounted next to each other, separated by a thin air layer as in the Glan-Foucault prism (Fig. 17.5a and Exercise 16.4) or by an appropriate cement as in the Nicol prism, the oldest device, invented by William Nicol in 1828 (Fig. 17.5b), and described below. The other type of polarizing prism allows both beams to go through, but they diverge at the exit, thus yielding two distinct, linearly polarized beams (Fig. 17.5c and 17.5d, and Exercise 16.6). The Nicol prism (sometimes called nicol) is an assembly of two calcite prisms (calcite is one of the crystal forms of calcium carbonate CaCO3 , also called Iceland spar because the ﬁrst crystals were found in Iceland), cut in a special way. Calcite has point group ¯3m. It is therefore uniaxial, and the optic axis is the 3-fold axis. Calcite crystals feature cleavage planes deduced from one another by the 3-fold symmetry around the optic axis. An Iceland spar crystal is cleaved along these three planes, forming a parallelepiped in which two sides (AB and AD) are equal and the third (AA ) is approximately three times longer than the two ﬁrst sides (Fig. 17.6a). These relationships were calculated so

Chapter 17 – Polarization of light by crystals

375

9 e

9

e

9

o

o

9 (a)

Canada balsam air

(b)

9

9 o

e

9

o 9

9

o

e

e

(c)

(d)

Figure 17.5: Schematic drawing of polarizing devices: (a) Glan-Foucault prism; (b) Nicol prism; (c) Wollaston prism; (d) Rochon prism. These prisms are made of calcite, a uniaxial negative crystal. A

A’

D’ F’

B C

A

A’ F

D

C’

A1

(a)

O9 Ro

B’ C

E

Re

O’ C’

A1

(b)

Figure 17.6: Nicol prism: (a) overall view; (b) principal section plane AA C C (perpendicular to the entrance face ABCD and containing the optical axis AA1 ). Only the extraordinary ray emerges from the exit surface. It is slightly shifted with respect to the incident beam, the direction of which is shown by a dotted line. that the diagonal plane AA C C be perpendicular to face ABCD used as the entrance face, and that it contain the optic axis AA1 . Plane AA C C is thus the principal section plane. The crystal is sawed along plane AFC F , perpendicular to the principal section plane. The two halves are then cemented together using a thin layer of Canada balsam, for which the index N is 1.55, a value between the ordinary index of calcite no = 1.6584 and its extraordinary index ne = 1.4864 (Fig. 17.6b). The incident beam is directed parallel to the large side AA of the prism, so that the incidence plane coincides with the principal section plane. The rays are drawn as in Figure 16.9c. The ordinary ray can be shown by calculation

376

Symmetry and Physical Properties of Crystals

to reach AC with incidence angle 75.7◦ , a value larger than the limiting angle,2 69.2◦ , corresponding to transition from the ordinary index of calcite to that of Canada balsam. It therefore undergoes total reﬂection. The index n for the extraordinary wave is equal to 1.53 (Exercise 16.5) for this orientation of the wave-vector. The extraordinary ray goes through the Canada balsam, then through the second prism, and emerges parallel to the incident beam and slightly shifted. The extraordinary ray is polarized parallel to the principal section plane. It is easy to rotate this polarization, just by rotating the prism around the incident beam.

17.4. Phase-shifting plates Birefringent plates are used to introduce a phase shift between two perpendicular components of an electromagnetic wave. Consider a uniaxial crystal plate, with parallel faces, cut so that the optic axis is in the plane of the plate (Fig. 17.7).

optic axis

no

O 9Eo

air crystal

x

ko ke

ne

Ee

9Eo

z

crystal air

Ee

Figure 17.7: Propagation of the ordinary and extraordinary rays through a phase-shifting plate, a uniaxial plate with the optic axis parallel to its faces Consider an incident beam perpendicular to the plate. The propagation geometry is then very simple. The ordinary and extraordinary wave-vectors are normal to the plate surface. The same applies for the directions of the ordinary and extraordinary rays in the crystal, and also in air at the exit of the plate. The index for the extraordinary ray is equal to ne . For this simple geometry where the ordinary and extraordinary rays are parallel to the corresponding wave-vectors, the electric ﬁeld vector E and induction vector D are parallel, and the polarization vector can be deﬁned by either of these vectors: we choose E. The polarization of the ordinary ray is perpendicular to the optic axis and that of the extraordinary ray is parallel to it. These two orthogonal 2. We recall that the limiting angle il for incidence of a wave on the surface separating a ﬁrst material, with index n1 , from a second material, with index n2 < n1 , corresponds to refraction angle 90◦ (sin il = n2 /n1 ). If the incidence angle is ≥ il , there is no refracted beam: the wave is totally reﬂected.

Chapter 17 – Polarization of light by crystals

377

directions are called the neutral lines of the plate. If we choose Oz parallel to the propagation direction and Ox parallel to the optic axis, the neutral lines of the plate are axes Ox and Oy. Consider an incident plane wave, the electric ﬁeld of which on the entrance face of the crystal (z = 0) has complex components (Sect. 17.2):

E1 exp −iωt . E2 exp iϕ exp −iωt In the plate, this wave gives rise to the ordinary wave, with polarization parallel to Oy, with index no , with the norm of its wave-vector k no , and to the extraordinary wave, with polarization parallel to Ox, with index ne , and with the norm of its wave-vector k ne . We recall that k = ω/c is the modulus of the wave-vector in vacuum. At a distance z from the entrance face, the wave has changed into: Ex = E1 exp i(k ne z − ωt) Ey = E2 exp iϕ exp i(k no z − ωt). At the exit of the plate with thickness e, the components Ey and Ex have an additional phase shift ψ such that ψ = k(no − ne )e, which can also be written: ψ=

2π (no − ne )e. λ

At the exit, the wave is given in Jones notation by:

E1 . E2 exp iϕ exp iψ The sign of ψ depends on the relative values of no and ne , or more precisely on the indices for each of the neutral lines. We thus distinguish the fast neutral line, parallel to the electric ﬁeld which propagates with the larger velocity and therefore the smaller index, and conversely the slow neutral line (smaller velocity and larger index). If Oy is the fast line, then the phase shift ψ is negative.

17.4.1. Half-wave plates These are plates where the thickness is such that the phase shift ψ is equal to (2p + 1)π, with p an integer. Assume the wave incident on the plate is linearly polarized, with components a and b along two orthogonal axes Ox and Oy, respectively parallel to the neutral lines of the plate.

a State before the plate: . b

a a State after the plate: = . b exp iπ −b

378

Symmetry and Physical Properties of Crystals

The vibration which, at the entrance to the plate, enclosed an angle θ with axis Ox such that tan θ = b/a now encloses an angle −θ (Fig. 17.1). A half-wave plate transforms a rectilinear vibration into another rectilinear vibration, symmetric of the ﬁrst one with respect to its neutral lines.

17.4.2. Quarter-wave plates These are plates whose thickness is such that the phase shift is equal to (p + 1/2)π with p an integer, i.e. ± π/2 modulo 2π. These plates make it possible to change linear polarization into circular polarization. Consider linearly polarized light (natural light after passage through a linear polarizer) such that its polarization direction is at 45◦ to the neutral lines of the plates, chosen as the Ox and Oy axes.

a The state before the plate is: a

a a and after the plate: = , a exp −iπ/2 −ia if the neutral line parallel to Oy is the fast line. After the plate, the polarization is right circular (Fig. 17.8). P

Plate

y

y

y F x

S x

x z

Figure 17.8: Schematic representation of a device providing right circular light starting from any incident polarization (generally an unpolarized beam). P is a linear polarizer. The plate is a quarter-wave plate. The fast F and slow S neutral lines are at an angle of 45◦ to the linear polarization transmitted by P. A left circular polarization would be obtained: either by rotating the polarizer by 90◦ or by leaving the polarizer in the same orientation and by rotating the plate by 90◦ , which exchanges the slow and fast axes of the plate and now introduces a phase shift of π/2. Quarter-wave plates are also used to analyse circular polarization. Consider a right-handed circularly polarized wave and let it go through a quarter-wave plate and then through a linear polarizer (called here analyzer) with a polarization direction at 45◦ to its neutral lines (Fig. 17.9). We choose axes Ox and Oy respectively parallel to the fast and slow neutral lines of the quarter-wave plate.

Chapter 17 – Polarization of light by crystals

379

The polarization direction of the linear analyzer makes an angle of 45◦ with the Ox axis. The Jones vector for the right-circularly polarized wave is:

a −ia

and the intensity of the wave is 2a2 . After the quarter wave plate which induces a phase-shift of π/2 between Oy and Ox components, the wave becomes

a a

.

It is linearly polarized with the polarization parallel to the polarization direction of the linear analyzer. The wave is completely transmitted by the polarizer and its intensity is 2a2 . If the incident wave had been a left-handed circularly polarized wave and if it was passed through the same device (quarter-wave plate and linear polarizer at 45◦ to the neutral lines), the transmitted intensity would have been zero. Such a device analyzes the intensity of the right-handed circular polarization. In contrast, the whole left-handed circularly polarized wave would have been transmitted through the same kind of device but with the direction of polarization of the linear polarizer at an angle of 135◦ with the Ox axis. A

Plate y

y S x

y F x

x z

Figure 17.9: Schematic representation of a device which totally transmits right-handed circular polarized radiation and stops left-handed circular polarization

17.5. Partially polarized waves and Stokes parameters The above sections dealt with perfectly monochromatic waves with perfectly deﬁned polarization state, i.e. totally polarized waves. For these waves, the end of the electric ﬁeld vector, at a given point, describes a perfectly deﬁned curve, an ellipse in the general case. This ellipse reduces to a circle for circularly polarized waves, and to a straight line segment for linearly polarized waves. We mentioned that, in contrast, classical light sources emit totally unpolarized waves (Sect. 17.1.4). The end of the electric ﬁeld vector moves randomly in the plane perpendicular to the propagation direction, and has no preferred orientation in this plane.

380

Symmetry and Physical Properties of Crystals

These two cases are the extreme situations of a totally polarized wave and a totally unpolarized wave. In many cases, we deal with a partially polarized wave, consisting of the superposition of monochromatic waves with various polarization states, obtained for instance through reﬂection or scattering, because these mechanisms aﬀect polarization in a way which depends on the incidence and scattering angles. We then deﬁne the polarization state of a wave propagating along direction Oz using the elements of the coherence matrix J:

< Ex Ex∗ > < Ex Ey∗ > Jxx Jxy = J= Jyx Jyy < E y Ex∗ > < Ey Ey∗ > where the angle brackets indicate that we are dealing with the average value of the quantity over all the waves in the beam. The polarization state of the wave is now deﬁned, using these matrix elements, through the Stokes parameters s0 , s1 , s2 and s3 [1] such that: s0 = Jxx + Jyy = < Ex Ex∗ > + < Ey Ey∗ > s1 = Jxx − Jyy = < Ex Ex∗ > − < Ey Ey∗ > s2 = Jxy + Jyx = 2 < Ex Ey∗ > s3 = − i(Jxy − Jyx ) = 2 < Ex Ey∗ > where stands for “real part of” and for “imaginary part of”. It is clear that s0 represents the intensity of the wave, and that s1 represents the diﬀerence between the intensies transmitted by polarizers with polarization directions respectively parallel to Ox and Oy. We now show that s2 represents the diﬀerence between the intensities transmitted by linear polarizers with polarization directions at 45◦ and 135◦ to Ox respectively. For a wave with Jones vector

Ex , Ey the amplitudes transmitted by these polarizers are respectively: √ E(45◦ ) = ( 2/2) (Ex + Ey ) for the polarizer at 45◦ and √ E(135◦ ) = ( 2/2) (Ex − Ey ) for the polarizer at 135◦ . The intensities are respectively: I(45◦ ) = 1/2 (Ex + Ey )(Ex∗ + Ey∗ ) = 1/2 (Ex Ex∗ + Ey Ey∗ + Ex Ey∗ + Ex∗ Ey ) I(135◦ ) = 1/2 (Ex − Ey )(Ex∗ − Ey∗ ) = 1/2 (Ex Ex∗ + Ey Ey∗ − Ex Ey∗ − Ex∗ Ey ) I(45◦ ) – I(135◦ ) = Ex Ey∗ + Ex∗ Ey = 2 (Ex Ey∗ ) and for a partially polarized wave: I(45◦ ) – I(135◦ ) = 2 < Ex Ey∗ > = s2 .

Chapter 17 – Polarization of light by crystals

381

Let us now show that s3 represents the diﬀerence between the intensities of the waves with right-circular and with left-circular polarization. We saw (Sect. 17.4.2) that the intensity of waves with right (respectively left) circular polarization can be measured using a device consisting of a quarter-wave plate and a linear polarizer with polarization direction at an angle of 45◦ (respectively 135◦ ) to the fast neutral line of the quarter-wave plate chosen as Ox axis. The amplitudes of the electric ﬁelds transmitted by these devices are noted E(π/2, 45◦ ) and E(π/2, 135◦ ) respectively. Similarly the transmitted intensities are noted I(π/2, 45◦ ) and I(π/2, 135◦ ) respectively. One gets: √ E(π/2, 45◦ ) = ( 2/2) (Ex + iEy ) and √ E(π/2, 135◦ ) = ( 2/2) (Ex − iEy ) where Ex and Ey are the components of the wave parallel to the directions of the neutral lines of the quarter-wave plate. Hence the transmitted intensities are: I(π/2, 45◦ ) = 1/2 (Ex + iEy )(Ex∗ − iEy∗ ), I(π/2, 135◦ ) = 1/2 (Ex − iEy )(Ex∗ + iEy∗ ). I(π/2, 45◦ ) − I(π/2, 135◦ ) = i (Ey Ex∗ − Ey∗ Ex ) = 2 (Ex Ey∗ ) and for a partially polarized wave: I(π/2, 45◦ ) − I(π/2, 135◦ ) = 2 < Ex Ey∗ > = s3 . The Poincaré coeﬃcients P1 , P2 and P3 are deﬁned as the Stokes parameters normalized by the intensity of the beam, so that: P1 =

s1 , s0

P2 =

s2 s0

and P3 =

s3 . s0

Thus P1 is the linear polarization rate for axis directions Ox and Oy, P2 that for directions at 45◦ and at 135◦ to axis Ox, and P3 the circular polarization rate (the relative diﬀerence between the intensities of right- and left-circularly polarized waves). A completely polarized wave is described by its Jones vector

a b exp iϕ where a and b are real numbers. Then its Stokes parameters are: s0 = a2 + b2 ,

s1 = a2 − b2 ,

s2 = 2 ab cos ϕ and s3 = 2 ab sin ϕ.

Thus, in this case, the four Stokes parameters are not independent, since s20 = s21 + s22 + s23 . For a partially polarized wave, this relation has no reason to be valid. It can be shown that in all cases s20 ≥ s21 + s22 + s23 , the equal sign applying to a totally polarized wave [1]. It can be shown also that the Stokes parameters of

382

Symmetry and Physical Properties of Crystals

a mixture of independent waves are sums of the respective Stokes parameters of the separate waves. The Stokes parameters of a totally unpolarized wave are such that s1 = s2 = s3 = 0. Considering a wave with given Stokes parameters and denoting by a single symbol s the four Stokes parameters s0 , s1 , s2 and s3 , one can write: s = s(1) + s(2) with and

s(1) = s0 − s21 + s22 + s23 , 0, 0, 0 s(2) = s21 + s22 + s23 , s1 , s2 , s3

s(1) represents the unpolarized part of the wave and s(2) the polarized part. Hence, the degree of polarization τ of the original wave, which is equal to the ratio of the intensity of the polarized part to the total intensity, is given by: Ipol s21 + s22 + s23 τ= = . Itot s0 Exercice 17.7 deals with an illuminating, albeit theoretical, partially polarized wave situation.

17.6. Exercises Exercise 17.1 Consider a plate of quartz (a uniaxial positive crystal, ne > no ), with parallel faces, cut so that the optic axis is parallel to the plate. A monochromatic parallel beam, with wavelength λ = 590 nm in vacuum, is incident on the plate, perpendicular to the plate. 1.

Determine the neutral lines of the plate. Choose an orthonormal axis system with Oz parallel to the incident beam and Ox and Oy parallel to the neutral lines of the plate.

2.

What phase shift does the plate introduce between the components parallel to Ox and Oy of an initially linear polarization? Determine the thickness e of the plate required to obtain a quarter-wave plate, then a half-wave plate. We have no = 1.544 and ne = 1.553.

3.

The incident beam is linearly polarized and its polarization is at 45◦ to the neutral lines of the plate. Show that, if the plate is a quarter-wave plate, the beam after the plate is circularly polarized. Is this a right- or a left-circular polarization? If it is right-circular (or left-circular), how should the device be changed to make it left-circular (or right-circular)?

4.

What do we obtain if we place across the path of this circularly polarized beam another quarter-wave plate, identical to the ﬁrst one, with its neutral lines parallel to those of the ﬁrst one?

Chapter 17 – Polarization of light by crystals 5.

383

What is the eﬀect of a quarter-wave plate on natural light?

Exercise 17.2 Consider a quartz plate (quartz is a uniaxial positive crystal, ne > no ), cut parallel to the optic axis, and set between two crossed polarizers, i.e. polarizers with perpendicular polarization directions. A monochromatic parallel beam (with wavelength λ in vacuum) is incident perpendicular to the plate. 1.

The polarization direction of the beam incident on the plate is at angle α to the fast neutral line of the quartz plate. Calculate, as a function of the phase shift ϕ introduced by the plate, the intensity I of the beam after the analyzer.

2.

Choose α = 45◦ . Determine the smallest thickness of the plate that makes it possible to obtain: i)

zero intensity,

ii) maximal intensity. 3.

α is still equal to 45◦ . The initial beam is now white (i.e. polychromatic), and we are interested in wavelengths in the visible range, 0.4 μm < λ < 0.8 μm. What wavelengths are extinguished after the analyzer if e = 0.2 mm? Assume that ne − no varies little with wavelength and is equal to 0.01.

Exercise 17.3 A parallel, monochromatic, linearly polarized beam is normally incident on a birefringent plate, the neutral lines of which are oriented at 45◦ to the rectilinear vibration. The phase shift introduced by the plate between the extraordinary vibration (// Oy) and the ordinary vibration (// Ox) is ϕ. 1.

Show that, after the plate, the vibration is elliptic, the axes of the ellipse being respectively parallel and perpendicular to the direction of the rectilinear vibration.

2.

Calculate the axis ratio of the ellipse.

Exercise 17.4 Using two linear polarizers with known polarization directions, how can the neutral line directions of a birefringent plate be determined? Exercise 17.5 Consider the Nicol prism described in Section 17.3. Figure 17.6b shows its principal section plane, coinciding with the plane of incidence. The angle (AC, AA1 ) between the optic axis and the entrance face is equal to 45◦ , angle (CA, CC ) is 71◦ and angle (C A, C C) is 22◦ . The ordinary and extraordinary indices of calcite are no = 1.6584, ne = 1.4864, and the index of Canada balsam is N = 1.55.

384

Symmetry and Physical Properties of Crystals

1.

Calculate the angle of incidence of the ordinary ray on AC . Show that this ray is totally reﬂected on the Canada balsam.

2.

Determine the direction of the wave-vector, the index and the polarization of the extraordinary ray. Show that it goes through the Canada balsam.

3.

What is the direction of the extraordinary ray in the prism? Show that the outgoing ray is very slightly shifted with respect to the incident beam.

Exercise 17.6 In view of a special optical application (generation of a wave with angular frequency 2ω starting from a wave with angular frequency ω, a process known as Second Harmonic Generation, SHG, see Complement 19C), we need to ﬁnd a direction of the wave-vector k in a birefringent crystal such that n(2ω) = n(ω). Because the index of a material varies with frequency, the solution can be found, in a uniaxial material, by associating the ordinary wave to one frequency and the extraordinary wave to the other one. For a crystal of KH2 PO4 (Potassium dihydrogen phosphate, KDP), which is uniaxial, ﬁnd the angle θ the wave-vector k must enclose with the optic axis so that ne (2ω) = no (ω), taking into account that n(2ω) > n(ω) and ne < no . Useful values are: for λ1 = 694.3 nm (corresponding to ω): no = 1.506 and ne = 1.466, for λ2 = λ1 /2: no = 1.534 and ne = 1.487. Exercise 17.7 1.

We consider a monochromatic wave with Jones vector

a ib in an axis system Oxy, where a and b are positive real numbers. What is, at a given point, the trajectory of the end of the electric ﬁeld vector of this wave? What is its circular polarization rate ?

2.

Same questions for a wave with Jones vector

b ia

3.

We consider the wave formed by the superposition of the two above waves. Determine the Stokes parameters for this wave and its degree of polarization.

References [1] M. Born and E. Wolf, Principles of Optics, 7th edn. (Cambridge University Press, Cambridge, 1999)

Chapter 18

Rotatory power and optical activity Going through some crystals rotates the linear polarization of incident radiation. This phenomenon, known as rotatory power or circular birefringence, is described by a diﬀerence in refractive index for right- and left-hand circular polarization. It is interpreted through the gyrotropy tensor, related to the space dependence of the permittivity tensor. The investigation of this tensor makes it possible to determine what point groups a crystal must belong to in order to feature this property.

18.1. Deﬁnition of the rotatory power of a material Rotatory power was discovered by François Arago in 1811 and Jean-Baptiste Biot in 1812. The ﬁrst theoretical interpretation was given by Augustin Fresnel in 1824. A material features rotatory power if it causes the plane of polarization of linearly polarized light1 to rotate. This property is distinctly diﬀerent from the previously discussed case of linear, or rectilinear, birefringence. It can exist in optically isotropic crystals (cubic crystals) and also in liquids or solutions. We will not deal with the rotatory power of liquids and solutions because they are outside the scope of this book, which focuses on crystalline solids. Also, the diﬀerences in refractive index involved in this phenomenon are much smaller than those corresponding to birefringence. Therefore, clearly evidencing rotatory power in anisotropic materials requires sending the beam parallel to the optic axis in uniaxial crystals (or to one of the two optic axes in biaxial crystals) in order to eliminate the eﬀect of birefringence.

1. The plane of polarization is the plane containing the wave-vector and the polarization vector, which is perpendicular to it. In a birefringent crystal, the polarization vector is the induction vector D, while in air, where the electric ﬁeld and induction are parallel, the description is based on the electric ﬁeld.

© Springer Science+Business Media Dordrecht 2014 C. Malgrange et al., Symmetry and Physical Properties of Crystals, DOI 10.1007/978-94-017-8993-6_18

385

386

Symmetry and Physical Properties of Crystals

Consider a material featuring rotatory power, for example a quartz plate in which the faces are perpendicular to the 3-fold axis. We illuminate this plate with a linearly polarized beam perpendicular to the plate. After going through the plate, the polarization has rotated by an angle α. This angle turns out experimentally to be proportional to the thickness e of the crystal. The rotatory power ρ is deﬁned by: α ρ= . (18.1) e If we exchange the entrance and exit faces of the plate, the polarization rotation angle α does not change sign. The sign of the rotation angle depends on the crystal, which may be either dextrogyre (rotation to the right) or levogyre (rotation to the left). This requires deﬁning what is meant by rotation to the right or to the left. A crystal is said to be dextrogyre if, for an observer looking at the source through the crystal, the plane of polarization of the light rotates to the right, i.e. clockwise (Fig. 18.1). crystal source

observer

Figure 18.1: Rotation of the induction vector to the right for an observer looking at the source The end of the polarization vector then describes, during propagation in the dextrogyre crystal, a left-handed helix (see Fig. 17.2). It was agreed to give positive values to α for dextrogyre materials. To indicate the order of magnitude of the rotatory polarization phenomenon, Figure 18.2 shows the value of the rotatory power ρ for quartz as a function of the wavelength of light in the visible range. We see that ρ is of the order of a few tens of degrees per millimeter of thickness traversed.

18.2. Fresnel’s interpretation Fresnel interpreted this phenomenon by showing that, if a material has diﬀerent refractive indices for right- and left-hand circular polarizations, then this material shows rotatory power. A linearly polarized electromagnetic wave can be split into two waves with equal amplitudes, one right-circular, the other left-circular. A wave propagating along Oz and polarized along Ox can be split, using the Jones notation (Sect. 17.2), in the following way:

1 1 1 1 1 + . = i 0 2 2 −i

Chapter 18 – Rotatory power and optical activity

387

60

[degree mm–1]

50 40 30 20 10 0 350

400

450

500

550

[nm]

600

650

700

Figure 18.2: Rotatory power of quartz as a function of wavelength The ﬁrst term represents a left-circular vibration, and the second term a right-circular vibration (Sect. 17.2), when using waves with the form [exp i(kz − ωt)]. If the index of the material for the right-circular vibration, nr , is diﬀerent from the index, nl , for the left-circular polarization, the initial wave, with wave-vector in air k0 = 2π/λ, becomes after propagating over a distance z in the crystal:

1 1 1 1 exp(ik0 nl z) + exp(ik0 nr z) i 2 2 −i

1 k0 (nl + nr )z = exp i 2 2

k0 (nr − nl )z k0 (nl − nr )z 1 1 + exp i . × exp i −i i 2 2 We set:

k0 (nl + nr )z k0 (nr − nl )z =ψ and = α . 2 2 We obtain a vibration:

1 cos α exp −iα + exp iα = exp iψ exp iψ i exp −iα − i exp iα sin α 2 i.e. a linearly polarized vibration, with polarization at an angle α with respect to the axis Ox which is parallel to the initial polarization. The plane of polarization of the vibration has rotated by an angle α , proportional to the thickness z of crystal traversed, and such that: α =

k0 (nr − nl )z π(nr − nl )z = . 2 λ

388

Symmetry and Physical Properties of Crystals

Here, α positive corresponds to the trigonometric sense, hence to a rotation to the left for an observer with the propagation vector of the incoming light pointing toward her, i.e. for an observer looking at the source: thus the crystal would be levogyre. Taking into account the convention on the sign of rotation deﬁned in the preceding section, α = −α, and the rotatory power ρ = α/z is equal to: π(nl − nr ) . (18.2) ρ= λ The material is dextrogyre if nl > nr , hence if the propagation velocity vr of right-circular polarized waves is larger than the propagation velocity vl of the left-circular polarized waves, and conversely for a levogyre crystal. Dextrogyre quartz has a rotatory power equal to 18.8◦ per mm for wavelength 632.8 nm (red helium-neon laser). Therefore nl − nr = 6.6 × 10−5 , a very small value compared to the birefringence of most crystals, which is on the order of 10−3 . For quartz, ne = 1.5533, no = 1.5442 and ne − no = 9 × 10−3 .

18.3. Interpretation of rotatory power through the inﬂuence of the local environment 18.3.1. Eﬀect of spatial dispersion Until now, we assumed that the electrical polarization at a point depends only on the electric ﬁeld at this point. Actually polarization can also depend on the local environment. This is described by a spatial dispersion term. The relation between E and D was, till now, described (see Eq. (16.22)) as: Em = ηmn

Dn . ε0

(18.3)

To account for spatial dispersion, we must add to Equation (18.3) a term proportional to the space derivatives of induction:

∂Dn 1 ηmn Dn + γmnp . (18.4) Em = ε0 ∂xp We seek a solution in the form of a plane sinusoidal wave: D = D0 exp i(k · r − ωt). We then have:

∂Dn = ikp Dn = iksp Dn ∂xp

where the si are the components of the unit vector parallel to k (k = ks). To simplify notations, we set βmnp = kγmnp , and Equation (18.4) becomes: Em =

1 (ηmn Dn + iβmnp sp Dn ). ε0

(18.5)

Chapter 18 – Rotatory power and optical activity

389

It can be shown [1] that tensor β, called the gyration tensor, is antisymmetric with respect to the ﬁrst two subscripts: βmnp = −βnmp . Among the 27 components βmnp , 9 (those of the form βiil ) are therefore zero, and the remaining 18 (of the form βijl with i = j) are pairwise opposite. There are thus 9 independent components. We deﬁne two-subscript components Gml through: 1 (18.6) Gml = δmij βijl 2 where δmij is the Levi-Civita symbol, or permutation tensor, which was deﬁned in Section 10.6.2 and which is shown to be an axial rank-3 tensor in Section 18A.2. We see for example that: 1 1 G11 = (δ123 β231 + δ132 β321 ) = (β231 − β321 ) or G11 = β231 = −β321 . 2 2 In the same way, G22 = β312 = −β132 ,

G12 = β232 = −β322 ,

etc.

It is easily shown (Sect. 18A.3) that performing a change in frame on the δmij ’s and the βijl ’s transforms the Gml ’s like the components of an axial rank-2 tensor. The axial rank-2 tensor [G] is called the gyrotropy tensor.2 We will see that rotatory power is described by the symmetrical part of [G] alone. Therefore all crystals for which [G] is non zero will be called optically active, whether the symmetrical part is zero or not. Those for which the symmetrical part of [G] is non zero (Sect. 18.5) will be said to feature rotatory power. We will also show (Sect. 18A.4) that relation (18.6) leads to: βijl = δijn Gnl and Equation (18.5) becomes: Em =

1 (ηmn Dn + iδmnj Gjp sp Dn ). ε0

(18.7)

We deﬁne axial vector g through its components gj = Gjp sp and:

g = [G]s.

(18.8)

Equation (18.7) becomes: Em =

1 (ηmn Dn + iδmnj gj Dn ). ε0

2. Some authors call [G] the gyration tensor. Here, we call it the gyrotropy tensor, in order to clearly distinguish it from [β], the gyration tensor (Eq. (18.6)).

390

Symmetry and Physical Properties of Crystals

The second term in the right-hand side is the m-th component of the cross product of vector D with vector g , and we can write: 1 E = ([η]D + iD × g ). (18.9) ε0 Optical activity introduces a purely imaginary term into the impermeability tensor.

We assumed, as in the preceding chapters (see Sect. 16.1), that the crystals are perfectly transparent, i.e. that absorption is zero. If it were not zero, absorption would correspond to a non-zero imaginary part in tensor [η]. The imaginary part which appears here in the relation between D and E has nothing to do with absorption. It introduces between E and D a phase-shift term which, as we will show further on, induces a diﬀerence between the indices of the material for the right- and left-circular polarizations which correspond to the eigenmodes. If absorption were to be taken into account, we would have to consider tensor [β] as complex, and to deal with its imaginary part. A complete treatment taking into account absorption can be found in the books by Agranovich and Ginzburg [2] and Barron [3].

18.3.2. Wave propagation in optically active crystals We saw (Eq. (16.15a)) that the propagation of a sinusoidal electromagnetic wave is described by the basic equation, reproduced here: D = ε0 n2 [E − s(s · E)]

(18.10)

where s is a unit vector parallel to the wave-vector. In Chapter 16, to obtain the propagation behavior of waves in a crystal, we associated to (18.10) relation E = [η]D/ε0 , which we must now replace with Equation (18.9). Since D is perpendicular to s (Eq. (16.10a), a result which is easily retrieved by writing the dot product of D and s in (18.10)), the search for vectors D that are solutions of (18.9) and (18.10) is simpliﬁed by projecting these equations onto a plane perpendicular to s. We choose Ox3 to be parallel to s, and we simplify the form of tensor [η] by choosing for Ox1 and Ox2 the directions of the axes of the ellipse along which the index ellipsoid intersects the plane perpendicular to s. In this coordinate system, tensor [η] can be written as: ⎞ ⎛ 0 η13 η1 ⎝ 0 η2 η23 ⎠ . η13 η23 η33 To simplify the analysis of the general case in what follows, we henceforth choose axis Ox1 such that η1 > η2 . Projecting (18.10) onto Ox1 and Ox2 provides: D1 = ε0 n2 E1 2

D2 = ε0 n E2 .

(18.11a) (18.11b)

Chapter 18 – Rotatory power and optical activity

391

Projecting (18.9) yields: D1 D2 + ig3 (18.12a) ε0 ε0 D2 D1 E2 = η2 − ig3 (18.12b) ε0 ε0 ⎞ ⎛ ⎞ ⎛ ⎞ ⎛ D1 D2 g3 g1 ⎠. −D1 g3 D × g = ⎝ D2 ⎠ × ⎝ g2 ⎠ = ⎝ 0 g3 D1 g2 − D2 g1 E1 = η1

because

Substituting in system (18.12) the values of E1 and E2 by their values as determined from system (18.11), we obtain: D1 D2 1 D1 = η1 + ig3 2 n ε0 ε0 ε0 1 D2 D2 D1 = η2 − ig3 . n2 ε0 ε0 ε0 This system can be written as: D 1 D =M n 2 0 0

with M=

η1 ig3 −ig3 η2

.

The solutions are the eigenvectors of matrix M . The eigenvalues λ of this matrix are the values of 1/n2 . They are obtained by solving equation: (η1 − λ)(η2 − λ) − g32 = 0.

(18.13)

Only the component g3 of g is used. The deﬁnition (18.8) of g makes it possible to write: gj = Gjp sp . Since, in the coordinate system we chose, s = (0, 0, 1), we deduce that g3 = G33 . Here the axis system, which we note R, is associated to the direction of the wave-vector. The gyrotropy tensor is in general deﬁned by its components Gij in an orthonormal axis system R associated to the crystal lattice. Let {aij } be the transformation matrix for going over from the orthonormal axis system R associated to the crystal lattice to the orthonormal axis system R associated to the wave-vector direction. We obtain: G33 = Δa3i a3j Gij = Δsi sj Gij where s1 , s2 and s3 are the components of vector s in the frame R associated to the crystal lattice. The determinant Δ of the transformation matrix is equal to 1 because frames R and R are both chosen to be direct. Finally: g3 = G33 = Gij si sj .

(18.14)

392

Symmetry and Physical Properties of Crystals

A special case: propagation along an optic axis This is the most frequent case in experiments, because then birefringence has no eﬀect, and optical activity is evidenced on its own. If s is parallel to an optic axis, then: 1 (18.15) η1 = η2 = 2 no where no is the index for propagation along the optic axis. For a uniaxial crystal, no is the ordinary index. Equation (18.13) has solutions λ = η1 ± g where, to simplify notations, we note g = g3 . The eigenvectors are then:

1 1 for λ = 2 = η1 + g, which is a right-circular polarized wave; −i n

1 1 for λ = 2 = η1 − g, which is a left-circular polarized wave (Sect. 17.2). i n We retrieve Fresnel’s assumption of two waves, right- and left-circular polarized, propagating with diﬀerent indices, nr and nl . Using (18.15), we obtain:

so that

1 1 1 1 = 2 +g and = 2 −g n2r no no n2l

1 2Δn Δ = − 3 = −2g n2 n

where Δn = nl − nr . We obtain Δn = nl − nr = gn3o and ρ=

π 3 gn λ o

g = Gij si sj ,

with

(18.16) (18.17)

where Gij , si , sj are components in the orthonormal axis system associated to the crystal. General case The eigenvalue Equation (18.13) has solution: λ± =

1 (η1 + η2 ) 1 ± [(η1 − η2 )2 + 4g2 ] 2 . 2 2

We recall that Ox1 was chosen such that η1 > η2 . We deﬁne τ such that: 1

[(η1 − η2 )2 + 4g2 ] 2 − [η1 − η2 ] = τ g, 2

Chapter 18 – Rotatory power and optical activity

393

and we note that |τ | ≤ 1 and τ g > 0. We obtain:

λ+ = η1 + τ g

and

λ− = η2 − τ g.

The associated eigenvectors are respectively:

1 τ and , −iτ i i.e. elliptical vibrations, the axes of which are the directions of the inductions which would propagate in the material if optical activity were neglected. We check that, for propagation along the optic axis, where η1 = η2 , we obtain τ = 1 if g > 0 and τ = −1 if g < 0, and thus right- and left-circular polarizations. Further, if g > 0, nr < nl (since τ = 1) and ρ is positive while, if g < 0, nr > nl and ρ is negative, in agreement with (18.16). As soon as the propagation direction deviates by a few degrees from the direction of the optic axis, η1 − η2 becomes large compared to g. We then ﬁnd τ g/(η1 − η2 ) so that τ 1. The waves have weak ellipticity. The major axes of these vibrations are parallel to the vibrations which would propagate if optical activity were neglected.

18.4. Eﬀect of crystal symmetry on the gyrotropy tensor The axial tensor [G] has no reason to be symmetric. However, (18.17) shows that only the symmetrical part of [G] is involved in rotatory power (18.16). The components of [G] with diﬀerent subscripts combine in (18.17) as, for example, (G12 +G21 )s1 s2 etc. However, it is interesting to begin by considering the whole tensor which represents the total optical activity, keeping in mind that only the symmetrical part of [G] is of interest for the rotatory power.

18.4.1. Centrosymmetric groups The axial rank-2 tensor [G] derives from the polar rank-3 tensor [β]. It is therefore clear that it is identically zero for all centrosymmetric crystal groups. This result can be retrieved directly using axial tensor [G]. The components Gij of an axial rank-2 tensor in an orthonormal coordinate system (Ox1 x2 x3 ) deduced from another orthonormal coordinate system (Ox1 x2 x3 ) through the transformation matrix {aij } are expressed as a function of the components Gij in the coordinate system (Ox1 x2 x3 ) through relation: Gij = Δaim ajn Gmn ,

(18.18)

394

Symmetry and Physical Properties of Crystals

where Δ is the determinant of matrix {aij } (see Eq. (18A.1)). If the crystal is centrosymmetric, a change from referential (Ox1 x2 x3 ) to the referential symmetric with respect to origin O must also leave the components of G unchanged, and Gij = Gij . But in this transformation aij = −δij and Δ = −1. Hence: Gij = −Gij . Finally

Gij = Gij = −Gij

and

Gij = 0.

18.4.2. Non-centrosymmetric groups We now examine some point groups using the direct inspection method. Group 2 We choose Ox3 to be parallel to the 2-fold axis. A rotation by π of the coordinate system (Ox1 x2 x3 ) around the 2-fold axis changes it into system (Ox1 x2 x3 ). The components of a vector transform according to x1 = −x1 ,

x2 = −x2

and x3 = x3 .

For a rotation, Δ = 1, hence [G] has form: 0 0

Group m We choose axis Ox3 perpendicular to the mirror. The operation of symmetry with respect to the mirror, when performed on the axis system, changes the components of a vector according to x1 = x1 ,

x2 = x2

and x3 = −x3 .

For mirror symmetry, Δ = −1, hence [G] has form: 0 0 0 0

Using the preceding result, we immediately see that, if we add to this mirror a 2-fold axis perpendicular to the mirror, hence parallel to Ox3 , all terms in this tensor are zero. This is no surprise since group 2/m is centrosymmetric. We note that the existence of a mirror implies that the trace of the matrix representing [G] is zero.

Chapter 18 – Rotatory power and optical activity

395

Group 4 We choose axis Ox3 parallel to the 4-fold axis. A rotation by π/2 of the coordinate system (Ox1 x2 x3 ) around the 4-fold axis changes it into system (Ox1 x2 x3 ), and the components of a vector transform according to x1 = x2 ,

x2 = −x1

and x3 = x3 .

For a rotation, Δ = 1 and [G] has form 0 0 0 0

where the empty circle connected to the full circle means that the two connected coeﬃcients have equal absolute values and opposite signs. We notice that here G12 = −G21 , so that [G] has an antisymmetric part. Rotatory power depends on the symmetric part of [G], so that the tensor representing the rotatory power has form: 0 0 0 0 0 0

Group 422 Group 422 deduces from group 4 by addition of a two-fold axis perpendicular to the 4-fold axis. One chooses the Ox3 axis parallel to the 4-fold axis and the Ox1 and Ox2 axes parallel to the two-fold axes. A rotation of the coordinate system (Ox1 x2 x3 ) by π around the 2-fold axis parallel to Ox1 changes it into system (Ox1 x2 x3 ), and the components of a vector transform according to x1 = x1 ,

x2 = −x2

and x3 = −x3 .

Δ = 1 and G12 = −G12 = G12 = 0. Tensor [G] is now symmetric and identical to the symmetric part of [G] for point group 4. Group 4mm Group 4mm deduces from group 4 by addition of a mirror parallel to the 4-fold axis. One chooses the Ox3 axis parallel to the 4-fold axis and the Ox1 and Ox2 axes perpendicular to the mirrors. A mirror symmetry normal to Ox1 transforms the coordinate system (Ox1 x2 x3 ) into system (Ox1 x2 x3 ), and the components of a vector transform according to x1 = −x1 ,

x2 = x2

and x3 = x3 .

396

Symmetry and Physical Properties of Crystals

For a mirror symmetry, Δ = −1 and G11 = G22 = G33 = 0 whereas G12 and G21 are not zero. The [G] tensor is now antisymmetric :

( ( 0 0 0 0 0 0

0

so that crystals belonging to class 4mm do not feature rotatory power. Table 18.1 gives the form of the gyrotropy tensor [G] for 18 out of the 21 noncentrosymmetric crystallographic groups. For the three other groups (¯43m, ¯ 62m and ¯6), all components are zero. For three groups (4mm, 3m and 6mm), tensor [G] is antisymmetric: thus they do not feature rotatory power, but they are optically active because of this antisymmetric [G] tensor. We showed (Sect. 10.6) that a rank-2 antisymmetric polar tensor is equivalent to an axial vector. In the same way, it can be shown that a rank-2 antisymmetric axial tensor is equivalent to a polar vector. The gyrotropy tensor of crystal classes 4mm, 3m and 6mm thus has only a vectorial part. It is interesting to note that all the crystal classes for which the [G] tensor involves a vectorial part (1, 2, m, mm2, 4, 4mm, 3, 3m, 6, 6mm) are just the pyroelectric classes. This vectorial part of the gyrotropy tensor can be evidenced using quite delicate reﬂectivity experiments. Table 18.2 gives the form of the symmetric part of the gyrotropy tensor or rotatory power tensor.

18.5. Rotatory power and chirality Table 18.3 gives examples of crystals featuring rotatory power, and the value of their rotatory power ρ (in absolute value) for a given wavelength. Wavelength 632.8 nm is that of the helium-neon laser. The crystals mentioned in this table belong to one of the crystal groups called enantiomorphic or chiral groups. These groups, featuring neither a mirror nor a center of symmetry, and, in a more general way, no roto-inversion, are groups 1, 2, 222, 3, 32, 4, 422, 6, 622, 23, 432. An object is said to be chiral if it is not superimposable with its image in a mirror. This is the case for a hand (in Greek: χειρ, hence the term chiral). The mirror image of a right hand is a left hand. In the same way, a helix is a chiral object: the mirror image of a right-handed helix is a left-handed helix, and conversely. Crystals belonging to these enantiomorphic groups can exist under two forms, called enantiomorphic, one dextrogyre, the other levogyre. Their structures deduce from each other through a mirror symmetry operation. For those whose space group has deﬁnite chirality because it includes a screw axis giving equivalent atom positions located on a right- or left-handed helix (31 and 32 for example),

Chapter 18 – Rotatory power and optical activity

397

Table 18.1: Form of the gyrotropy tensor [G ] Triclinic 1 Monoclinic

2

0 0

2 Ox 3

2 Ox 2

0 0

m

m Ox 3

0 0 0 0

m Ox 2 0

Orthorhombic 222

0 0 0 0 0 0 0 0

Tetragonal 4

Rhombohedral and Hexagonal

0 0 0 0 0 0 0

3, 6 0 0

Cubic 23, 432 Equal components

0

0 0 0

0

mm2

0

0 0 0 0 0 0

422

0 0 0 0 0 0

– 42m 2 Ox1

0 0 0 0 0 0 0

32, 622 2 Ox1

0 0 0 0 0 0

0 0 – 4

0 0

0 0

0

4mm

3m, 6mm m Ox 1

0 0 0 0 0 0

0

0 0 0 0 0 0

0 0 0 0 0 0 Components with equal absolute values but opposite signs

the space groups of crystals of these two enantiomorphic forms are diﬀerent. For example, right-handed quartz has space group P31 21 and left-handed quartz P32 21. The connection between the chirality of the crystal structure and the sign of the rotatory power has long been discussed, and it is no trivial matter. Rotatory power is due to the most polarizable atoms. If these atoms are not in equivalent crystal sites, they can actually form pseudo-helices with chirality opposite to the chirality of the crystal axis, as was shown by A.M. Glazer and K. Stadnicka [4]. The same authors showed that, in crystals where the screw axes have no deﬁnite chirality, such as 63 or 21 (Sect. 7.2.1), the most polarizable atoms form pseudo-helices with given chirality for a given enantiomorph. It can be noticed that the trace of the matrix representing tensor [G] in enantiomorphic classes is non zero whereas for the other crystals featuring rotatory power the trace is zero. This is not surprising since we already noticed that, for crystal classes with a mirror symmetry the trace of [G] is zero (see group m in Sect. 18.4.2).

398

Symmetry and Physical Properties of Crystals

Table 18.2: Form of the symmetrical part of the gyrotropy tensor [G ] for the various point groups. Only the coeﬃcients on the diagonal and in the part above it are represented. Triclinic 1 Monoclinic

0 0

2

2 Ox 3

m

m Ox 3

0 0 0

0

2 Ox 2

m Ox 2

0 0

0 0

0 222

0 0 0

mm2

4, 422

0 0 0

– 4

3, 32, 6, 622

0 0 0

23, 432

0 0 0

Orthorhombic

Tetragonal

Rhombohedral and Hexagonal

0

Cubic

Equal components

0

0 0 0 0 0 0 0

– 42m 2 Ox1

0 0 0 0

Components with equal absolute values but opposite signs

Table 18.3: Values of the rotatory power ρ of some crystals Material

Quartz (SiO2 )

Point group 32

Space group P31 21

Wavelength (nm)

ρ (degree . mm−1 )

643.8

18

274.0

122.1

Berlinite (AlPO4 )

32

P31 21

632.8

14.6

Cinnabar (HgS)

32

P31 21

632.8

320

NaBrO3

23

P21 3

632.8

1.65

NaClO3

23

P21 3

632.8

2.44

α−LiIO3

23

P63 2

632.8

86.7

Chapter 18 – Rotatory power and optical activity

399

While rotatory power is possible for all crystals belonging to an enantiomorphic group, the converse property is not true: belonging to an enantiomorphic group is not a necessary condition for a crystal to feature rotatory power. This is shown on Table 18.2, where non-enantiomorphic groups m, mm2, ¯4 and ¯42m are seen to feature rotatory power. However, the rotatory power of these crystals is often diﬃcult to measure, because they do not necessarily feature rotatory power along the optical axis, and it is then necessary to measure a rotatory power combined with birefringence. The sign of the rotatory power in these crystals depends on the direction of the incident beam, and the crystal is dextrogyre or levogyre depending on this direction. Take the example of a crystal with point group mm2, for which tensor [G] has only one non-zero component, G12 .3 From (18.16) and (18.17), its rotatory power is proportional to G12 s1 s2 . If the optic axes for this crystal are in plane (Ox1 x2 ), the sign of the rotatory power is positive along one of the axes, and negative along the other one, since the product s1 s2 changes sign from one optic axis to the other. This is the case for sodium nitrite NaNO2 in its ferroelectric phase (T < 163◦ C), where rotatory power was measured for wavelength 632.8 nm (Fig. 18.3). Along one of the optic axes, the rotatory power is 15.7◦ /mm, while it has the same value but opposite sign along the other optic axis. M optic axis

optic axis b a

M

Figure 18.3: Plane (a, b), and therefore (Ox 1 , Ox 2 ) for a crystal of sodium nitrite (NaNO2 ). The angle α between the optic axes and one of the two mirrors M is equal to 33◦ . These results are interpreted by taking into account the positions of the ions in the unit cell: they form a left-handed helix along an axis approximately parallel to one of the optic axes, and form a right-handed helix along an axis approximately parallel to the other optic axis. The two optic axes deduce from each other through a mirror operation which changes the right-handed helix into a left-handed helix and vice-versa. In contrast, if the optic axes are in the plane perpendicular to Ox1 or to Ox2 (a frequent case), the rotatory power along the optic axes is zero (s1 or s2 being equal to zero), and the rotatory power becomes very diﬃcult to measure. 3. We recall that, for an orthorhombic crystal with point group mm2, the basis vector c (and thus axis Ox3 ) is chosen parallel to the 2-fold axis.

400

Symmetry and Physical Properties of Crystals

18.6. Absorption and conclusion We neglected absorption, which is extremely weak in transparent crystals at the wavelengths in the visible range considered here. We thus neglected the imaginary part of the index. The real and imaginary parts of the index are not independent. They are connected through integral relations (involving integration over the whole frequency range) known as the Kramers-Kronig relations (see [5]). As a consequence, a diﬀerence in index for two diﬀerent polarizations leads to a notable diﬀerence in absorption near an absorption edge: this is dichroism. The birefringence discussed in Chapter 16 corresponds to a difference in index for two orthogonal linear polarizations. There is therefore a diﬀerence in absorption for these two polarizations, hence linear dichroism. The rotatory power is due to a diﬀerence in index for the right-circular and left-circular polarizations, which leads to a diﬀerence in absorption for these two polarizations, hence circular dichroism. In the X-ray range, where crystals are not transparent, optical activity was experimentally evidenced recently, through dichroism measurements for natural rotatory power [6], and through reﬂectivity measurements for the vectorial part of [G] [7]. We showed that, among the 21 non-centrosymmetric crystal classes, 18 are optically active. Out of these 18 classes, 15 feature rotatory power. Among these 15 classes, 11 are enantiomorphic, which means that crystals in these classes can exist under two diﬀerent, mutually symmetric forms, one dextrogyre and the other levogyre. We have seen that the gyrotropic tensor of enantiomorphic classes has non-zero trace whereas, for the 4 non-enantiomorphic classes, the trace of [G] is zero. For the 3 optically active classes which do not feature rotatory power, the axial tensor [G] is antisymmetric and can be represented by a vector. This distinction between enantiomorphic crystals, non-enantiomorphic crystals which nevertheless feature rotatory power, and optically active crystals just on the basis of the vector part of [G], was ﬁrst introduced by Jerphagnon and Chemla in 1976 [8]. These authors split the symmetric part of [G] into the sum of an isotropic tensor (proportional to the unit tensor), which they note [A], and a tensor [D]. Thus the gyrotropy tensor [G] is the sum of [A], [D] and the vector part V (equivalent to the antisymmetric part of [G]). For enantiomorphic crystals, [A] is not zero, all crystals featuring rotatory power have [A] + [D] non zero, and optically active crystals with no rotatory power have only V non zero.

Chapter 18 – Rotatory power and optical activity

401

Complement 18C. Magnetic optical rotation The magneto-optical eﬀects can be deﬁned as the eﬀects of a magnetic ﬁeld on the propagation of an electro-magnetic wave, and can be described through the change in the high-frequency susceptibility tensor and refractive indices of a material due to the magnetic ﬁeld. The Faraday magneto-optical eﬀect, or magnetic gyrotropy, is the best-known member of this family. It concerns visible and near-visible light, but is now also an active ﬁeld of research, using synchrotron radiation, in the X-ray spectral range. The Faraday eﬀect, discovered in 1845, consists in the rotation4 of the plane of polarization of linearly polarized light under the inﬂuence of a magnetic ﬁeld B or magnetization parallel to the propagation direction. It is thus reminiscent of natural rotatory power, discussed in this chapter. It too can be conveniently described through the diﬀerence in the refractive indices, hence the diﬀerent phase velocities, associated to the right- and left-hand circular polarization states which are the eigenmodes. In materials with no spontaneous magnetization, such as dia- or paramagnets, the rotation α is proportional to the modulus of the magnetic ﬁeld B and to the length of material d traversed by the light beam: α = kV Bd,

where kV is the Verdet “constant”, a material-dependent function of the temperature and wavelength, with values on the order of 101 rad T−1 m−1 . In materials with spontaneous magnetization, typically ferrimagnets which are fairly transparent in the visible and near infra-red range, the eﬀect of the magnetic ﬁeld is primarily to steer the distribution of local magnetization in the various domains (see note in Complement 8C), favoring those with direction close to the ﬁeld, and tending toward saturation. The rotation is then α = θF d, with θF the rotation per unit length for magnetization parallel to the magnetic ﬁeld. Values are on the order of 104 degree cm−1 for substituted iron garnets (BiRGa)Fe5 O12 where R is a rare-earth element. An essential feature that distinguishes magnetic and natural rotatory power is the behavior under reversal of the propagation direction of light. After two successive passes in opposite directions through a sample, the eﬀect of spontaneous rotatory power cancels out. In the case of magneto-optical activity, in contrast, the rotation of the plane of polarization is doubled (Fig. 18C.1). This is usually designated as non-reciprocity, and is related to the non-invariance under time reversal (see Complement 8C) featured by a system with magnetization.

4. The rotation is actually complemented by the appearance of ellipticity.

402

Symmetry and Physical Properties of Crystals E0

B

E1

B E2

(a)

E1

(b)

Figure 18C.1: (a) Faraday rotation in an isotropic material (for example

a liquid) submitted to magnetic ﬁeld B: the polarization of the light is rotated by the angle α between E0 and E1 ; it is here counterclockwise as seen by an observer looking at the light source. With just the magnetic ﬁeld reversed, the rotation of the polarization becomes −α, clockwise for the observer. (b) The propagation direction is reversed, but not the magnetic ﬁeld: the rotation of the polarization is now clockwise for the observer (looking at the source, hence to the right), and therefore counterclockwise when looking along the propagation direction. Hence the overall rotation with respect to the laboratory frame, after two passes in opposite directions, is 2α. The Faraday eﬀect in ferrimagnets has applications such as magneto-optical isolators (preventing light from propagating in one direction), magnetic ﬁeld sensors, or the observation of magnetic domains and of magnetic ﬁeld maps.

Further reading E. du Trémolet de Lacheisserie, D. Gignoux and M. Schlenker (ed.), Magnetism, vol. 1: Fundamentals (Springer Verlag, New York and Heidelberg, 2005), chap. 13

Chapter 18 – Rotatory power and optical activity

403

Appendix 18A. Axial tensors, or pseudo-tensors 18A.1. Deﬁnition of axial tensors, or pseudo-tensors In Chapter 9, we deﬁned a rank-n tensor as a mathematical object having, in a given orthonormal frame, 3n components (if considering three-dimensional space) which, in a change of orthonormal frame, transform like the product of n components of vectors. This deﬁnition corresponds to polar tensors. Consider for example a rank-3 tensor, with components Tijk in a given frame. After a change in frame characterized by transformation matrix A, with coeﬃcients aij , such that: the new components of this tensor become Tmnp Tmnp = ami anj apk Tijk .

A polar vector is a rank-1 tensor. We saw (Eq. (10.13)) that the components wi of an axial vector, or pseudo such that: vector, transform in a change of orthonormal frame into wm = Δami wi wm

where Δ is the determinant of the transformation matrix, +1 for direct (or proper) transformations, and −1 for indirect (or improper) transformations. More generally, pseudo-tensors (or axial tensors) of rank n are deﬁned as mathematical objects having, in a given orthonormal frame, 3n components which, in a change of frame, transform like the product of n components, multiplied by the determinant of the matrix transforming one frame into the other. For example, a rank-3 axial tensor with components Vijk in a given frame will, in another frame deduced from the previous one through the transformation such that: matrix A, have components Vmnp = Δami anj apk Vijk . Vmnp

(18A.1)

18A.2. Levi-Civita tensor, or permutation tensor In Section 10.6.2, we deﬁned the Levi-Civita symbol, δijk , such that, whatever the coordinate system used, δijk = 0 if at least two of the subscripts i, j and k are equal, δijk = 1 if the permutation ijk is direct (123, 231, 312), δijk = −1 if it is indirect (132, 213, 321). To show that this symbol is an axial tensor, we consider ﬁrst the polar tensor of rank 3, εijk , deﬁned in a given system of axes, with basis vectors e1 , e2 and e3 through: εijk = 0 if two of the subscripts i, j or k are equal, εijk = 1 if the circular permutation ijk is direct (123, 231, 312),

404

Symmetry and Physical Properties of Crystals εijk = −1 if it is indirect (132, 213, 321).

In another orthonormal axis system, with basis vectors e1 , e2 and e3 , with transformation matrix {aij }, these components become: εmnp = ami anj apk εijk = am1 (an2 ap3 − an3 ap2 ) + am2 (an3 ap1 − an1 ap3 ) + am3 (an1 ap2 − an2 ap1 ) = [am1 (en × ep )1 + am2 (en × ep )2 + am3 (en × ep )3 ] = em · (en × ep ) = (em , en , ep ).

We thus see that: εmnp = 0 if two of the subscript m, n, p are equal, εmnp = Δ for mnp = 123, 231 and 312, εmnp = −Δ for mnp = 132, 213 and 321, where Δ is the determinant of the transformation matrix. This result shows that the Levi-Civita symbol, which retains the same value irrespective of coordinate changes, must therefore transform in a change of coordinate system in the following way: = Δami anj apk δijk . δmnp

It is therefore a rank-3 pseudo-tensor, or axial tensor, called the permutation tensor.

18A.3. The gyrotropy tensor [G] is a rank-2 axial tensor We show that the gyration tensor Gml is a rank-2 axial tensor by investigating how it transforms in a coordinate system change with transformation matrix {aij }. By deﬁnition (18.6), 1 Gml = δmij βijl 2 where δmij is the permutation tensor, a rank-3 axial tensor, and βijl a polar rank-3 tensor. The new components Guv are such that: Guv =

1 1 δ β = Δaum ain ajp δmnp aik ajl avw βklw . 2 uij ijv 2

From Equation (9.10), ain aik = δnk and ajp ajl = δpl , hence we can write: 1 1 Guv = Δδnk δpl aum avw δmnp βklw = Δaum avw δmnp βnpw = Δaum avw Gmw . 2 2 This shows that [G] is a rank-2 axial tensor.

Chapter 18 – Rotatory power and optical activity

405

18A.4. Relation between tensors [G] and [β] We calculate the product δijn Gnl by using the deﬁnition (18.6) of Gnl . δijn Gnl =

1 δijn δnmp βmpl . 2

For given i, j and n such that δijn = 0, the only non-zero products δijn δnmp are δijn δnij equal to 1, and δijn δnji equal to −1. Hence: δijn Gnl =

1 (βijl − βjil ) = βijl . 2

We obtain the relation: βijl = δijn Gnl .

406

Symmetry and Physical Properties of Crystals

References [1] L.D. Landau, E.M. Lifshitz and L.P. Pitaevskii, Course of Theoretical Physics, vol. 8, Electrodynamics of Continuous Media, 2nd edn. (Elsevier, Oxford, 1984) [2] V.M. Agranovich and V.L. Ginzburg, Crystal Optics with Spatial Dispersion, and Excitons, 2nd edn. (Springer-Verlag, 1984) [3] L. Barron, Molecular Light Scattering and Optical Activity, 2nd edn. (Cambridge University Press, 2004) [4] A.M. Glazer and K. Stadnicka, J. Appl. Cryst. 19, 108–122 (1986) [5] J.D. Jackson, Classical Electrodynamics, 3rd edn. (Wiley, 1998) [6] J. Goulon et al., X-ray natural circular dichroism in uniaxial gyrotropic single crystals of LiIO3 , J. Chem. Phys. 108, 6394–6403 (1998) [7] J. Goulon et al., Vector part of optical activity probed with X-rays in hexagonal ZnO, J. Phys. Condens. Matter 19, 156201–156219 (2007) [8] J. Jerphagnon and D.S. Chemla, J. Chem. Phys. 65, 1522–1529 (1976)

Optical activity in crystals,

Chapter 19

Electro-optical and elasto-optical eﬀects This chapter introduces various eﬀects through which the refractive index of a crystal (directly related to its permittivity tensor) can be altered through an external ﬁeld, such as a static electric ﬁeld or a strain. These changes to the index induced by an external, freely tailored ﬁeld, have many applications. Some of these are introduced as the various eﬀects are discussed.

19.1. Introduction We saw that the optical properties of a crystalline material are directly related to the tensor of electrical impermeability [η]. This tensor is the inverse of the permittivity tensor [ε], which is related to the electrical susceptibility tensor [χ] by relation: [ε] = ε0 ([E] + [χ]) where [E] is the identity tensor. The electrical susceptibility [χ] describes the appearance of a polarization P (electric dipole moment per unit volume) under the action of the electric ﬁeld E of the optical wave incident on the crystal. In Chapter 16, which deals with crystal birefringence, we restricted the Maclaurin expansion of the polarization P of the material as a function of the electric ﬁeld E with angular frequency ω, to the linear term: P(ω) = ε0 [χ]E(ω).

(19.1)

We then showed (Chap. 18) that optical activity is due to the inﬂuence of the local environment on the susceptibility, leading, in the expansion of P as a function of E, to an additional term, proportional to the spatial derivatives of the components of the electric ﬁeld: ∂Ej (ω) Pi (ω) = χij Ej (ω) + χijk . ε0 ∂xk © Springer Science+Business Media Dordrecht 2014 C. Malgrange et al., Symmetry and Physical Properties of Crystals, DOI 10.1007/978-94-017-8993-6_19

(19.2)

407

408

Symmetry and Physical Properties of Crystals

The susceptibility can also be inﬂuenced by the application of a static electric ﬁeld Es which contributes to the expansion (19.2) an additional term of the form χijk Ejs Ek (ω): ∂Ek (ω) Pi (ω) = χij Ej (ω) + χijk + χijk Ejs Ek (ω) + . . . ε0 ∂xj

(19.3)

The expansion can be continued by adding a term depending on the square of the applied static electric ﬁeld, and possibly other terms related to the inﬂuence on the susceptibility of other sorts of applied ﬁelds, such as a strain or a stress or a static magnetic ﬁeld. The existence of these additional terms in the expansion of the susceptibility leads to a dependence of the impermeability tensor [η] on these external applied ﬁelds. This means that optical propagation is coupled, for example, with an applied electric ﬁeld (electro-optical eﬀects), a strain or stress (elasto-optical eﬀects), or a magnetic ﬁeld (magneto-optical eﬀects). These couplings make it possible to alter optical propagation in crystals through these external ﬁelds, and they give rise to many applications. We restrict discussion to a few examples which give insight on how to deal with these couplings. Section 19.2 introduces electro-optical eﬀects, and Section 19.3 introduces elasto-optical eﬀects, which are also called acousto-optical eﬀects when the deformation results from the application of an acoustic wave.

19.2. Electro-optical eﬀects Applying a static electric ﬁeld Es to a crystal alters the dielectric impermeability tensor [η]. We can write: ηij (E) − ηij (E = 0) = Δηij = rijk Ek + zijkl Ek El + . . . To simplify notations, we replaced in this expression Es by E, because there is no ambiguity with the electric ﬁeld E(ω) of the optical wave, since E(ω) is not involved in this expression for [η]. The second-order term is much smaller than the ﬁrst-order one. Therefore we investigate the linear term ﬁrst. The quadratic term is evidenced when the linear term is zero. The coeﬃcients rijk are the components of a rank-3 tensor since they relate rank-1 tensor E with rank-2 tensor [η]. In the same way, coeﬃcients zijkl are the components of a rank-4 tensor.

19.2.1. Linear electro-optical eﬀect, or Pockels eﬀect General properties The changes induced on the tensor by a static electric ﬁeld E are small, even for rather strong applied ﬁelds (104 V cm−1 ). They are of interest only when they bring about a qualitative change to tensor [η]: for instance when a cubic,

Chapter 19 – Electro-optical and elasto-optical eﬀects

409

therefore optically isotropic, crystal becomes optically anisotropic (induced birefringence), or when a uniaxial crystal becomes biaxial. This change then has the advantage that it can be modulated by altering the amplitude of the electric ﬁeld. The linear eﬀect is described by: Δηij = rijk Ek where the rijk are the coeﬃcients of the electro-optical Pockels rank-3 tensor, [r]. Tensor [Δη], the diﬀerence between two symmetric tensors, is symmetric, and the two-subscript notation involving i and j can be replaced by a singlesubscript notation, as was done for the stress tensor [T ]. We then obtain six components Δηα , where α ranges from 1 to 6, and tensor rijk can be written with two subscripts. We note that, in contrast to the piezoelectric tensor (Sect. 15.3.2), no doubling occurs when going over from the rijk to the rαk . We have Δη23 = r23k Ek and Δη32 = r32k Ek , and the symmetry of [Δη] leads to r23k = r32k . We can write:

Δη4 = Δη23 = Δη32 = r4k Ek

with r4k = r23k = r32k , so that: Δηα = rαk Ek . In matrix notation, the vectors with components Δηα and Ek are column vectors, and the components rαk form a matrix with 6 rows and 3 columns, as for the inverse piezoelectric eﬀect. ⎞ ⎛ ⎞ ⎛ Δη1 r11 r12 r13 ⎜ Δη2 ⎟ ⎜ r21 r22 r23 ⎟ ⎛ ⎞ ⎟ ⎜ ⎟ ⎜ E1 ⎜ Δη3 ⎟ ⎜ r31 r32 r33 ⎟ ⎟ ⎜ ⎟ ⎝ E2 ⎠ . ⎜ ⎜ Δη4 ⎟ = ⎜ r41 r42 r43 ⎟ ⎟ ⎜ ⎟ ⎜ E3 ⎝ Δη5 ⎠ ⎝ r51 r52 r53 ⎠ Δη6 r61 r62 r63 The eﬀect of crystal symmetry on the number of independent components is the same as for the piezoelectric tensor. We therefore refer to Table 15.2, using the transposed matrices (Tab. 19.1a and 19.1b) and taking into account the fact that rαk = rijk for α = 4, 5, 6 whereas diα = 2dijk . We recall that material rank-3 tensors are zero for all centrosymmetric crystals. The order of magnitude of the non-zero components of tensor [r] is 10−12 m V−1 , thus picometres per volt (pm V−1 ).

410

Symmetry and Physical Properties of Crystals

Table 19.1a : Form of the matrices representing the electro-optical Pockels tensor (linear eﬀect) for various point groups 1

Triclinic

Monoclinic

2 2 Ox2

0 0 0

m 2 Ox3

0 0

0 0 0 0

0

0 0

0 0

Orthorhombic

Tetragonal

0 0

0 0

0 0

0

0 0

0

0

222

mm2

0 0 0 0 0 0 0 0 0 0 0 0 0 0 0

0 0 0 0 0 0 0 0 0 0 0 0 0

4

– 4

422

4mm

0 0 0 0 0 0 0 0 0 0 0

0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0

0 0 0 0 0 0 0 0 0 0 0 0 0

0 0 0 0 0 0 0 0 0 0 0

m Ox3

0 0 0 0

0 0

m Ox2

Equal components Components with equal absolute values but opposite signs

0 0 0 0 0

– 42m (2 Ox1)

0 0 0 0 0 0 0 0 0 0 0 0 0 0 0

Chapter 19 – Electro-optical and elasto-optical eﬀects

411

Table 19.1b : Form of the matrices representing the electro-optical Pockels tensor (linear eﬀect) for various point groups (continued) 3

Rhombohedral

32

3m

2 Ox1

0 0 0 0 0 0 0 0 0

0 0 0 0 0 Hexagonal

6

0 0 0 0 0 0 0 0 0 0 0

0 0 0 0

m Ox1

0 0

0 0 0 0 0 0 0 0

– 6

622

0 0 0 0 0 0 0 0 0 0 0 0

0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0

– 62m m Ox2

0 0 0 0 0 0 0 0 0 0

0 0 0 0 0 0

0 0 0 0

0 0 0 0 0 0 0 0

0 0 0 0 0

0 0 0 0 0

0 0 0 0 0

432

– 43m, 23

0 0 0 0 0 0

0 0 0 0 0 0

0 0 0 0 0 0

0 0 0 0 0 0 0 0

6mm

m Ox1

Cubic

m Ox2

0 0

0 0 0 0 0 0 0 0 0 0 0 0 0 0 0

Equal components Components with equal absolute values but opposite signs

412

Symmetry and Physical Properties of Crystals

Example of a cubic crystal with point group 23 This corresponds to crystals of sodium bromate NaBrO3 or of sodium chlorate NaClO3 . Tensor [r], expressed in the crystallographic axis system, has only three nonzero components which are equal to one another, r41 = r52 = r63 . Consider a crystal plate of NaBrO3 (or NaClO3 ), with faces perpendicular to one of the 2-fold axes, chosen as Ox3 . We apply an electric ﬁeld perpendicular to the plate (Fig. 19.1a). n + r41 En3/2

x2 b

k

n – r41 En3/2

x’2

x1 a c

x2

x’1 b

x3

O

a

x1

E

(a)

(b)

Figure 19.1: (a) Schematic representation of optical propagation in a crystal of NaClO3 submitted to an electric ﬁeld parallel to basis vector c; (b) directions of the neutral lines of the plate (dotted lines) We have: ⎛ ⎜ ⎜ ⎜ ⎜ ⎜ ⎜ ⎝

Δη1 Δη2 Δη3 Δη4 Δη5 Δη6

⎞

⎛

⎟ ⎜ ⎟ ⎜ ⎟ ⎜ ⎟=⎜ ⎟ ⎜ ⎟ ⎜ ⎠ ⎝

0 0 0 0 0 0 0 0 0 0 r41 0 0 r41 0 0 0 r41

⎞

⎛

⎟⎛ ⎞ ⎜ ⎟ ⎜ 0 ⎟ ⎜ ⎟⎝ 0 ⎠ = ⎜ ⎟ ⎜ ⎟ E ⎜ ⎠ ⎝

0 0 0 0 0 r41 E

⎞ ⎟ ⎟ ⎟ ⎟. ⎟ ⎟ ⎠

[Δη] has one non-zero component, and the electrical impermeability tensor [η] becomes: ⎞ ⎛ r41 E 0 η0 ⎝ r41 E η0 0 ⎠ 0 0 η0 where η0 is the value for zero electric ﬁeld, η0 = 1/n2 (Eq. (16.24)), where n is the index of the crystal without electric ﬁeld. The crystal is now birefringent. Axis Ox3 , parallel to one of the basis vectors of the cubic unit cell of the crystal (c on Fig. 19.1a) and to the applied electric ﬁeld, is a principal axis of the tensor. In an axis system (Ox1 x2 x3 ) rotated by 45◦ around axis Ox3 ,

Chapter 19 – Electro-optical and elasto-optical eﬀects tensor [η] becomes:

⎞

⎛

1 ⎜ n2 + r41 E ⎜ ⎜ 0 ⎜ ⎝ 0

413

0 1 − r41 E n2 0

0 ⎟ ⎟ 0 ⎟ ⎟. 1 ⎠ n2

Axes Ox1 and Ox2 are principal axes. The principal values of tensor [η] are the reciprocals of the squares of the indices ni which deﬁne the index ellipsoid (16.24), hence: 1 1 = 2 + r41 E 2 n n1

and

1 1 = 2 − r41 E. 2 n n2

Suppose we send onto the crystal a plane electromagnetic wave with wavevector k perpendicular to the plate, hence parallel to the electric ﬁeld (Fig. 19.1a). The components of the electric ﬁeld of the wave along Ox1 and Ox2 propagate with diﬀerent indices n1 and n2 (Fig. 19.1b). The diﬀerence Δn = n2 − n1 is easily calculated, because the change induced by the electric ﬁeld is very small. We obtain:

1 Δn (19.4) Δ = −2 3 = −2r41 E n2 n whence we deduce:

Δn = n2 − n1 = n3 r41 E.

The crystal plate has become birefringent, and its birefringence is proportional to the value of the applied electric ﬁeld. Its neutral lines are parallel to Ox1 and Ox2 , thus at 45◦ to vectors a and b. Example of a tetragonal crystal with point group ¯ 42m: a crystal of KDP (potassium dihydrogen phosphate KH2 PO4 ) We consider a plate of KDP in which the faces are perpendicular to the optic axis (¯4 axis parallel to c), and an incident wave normal to the plate (Fig. 19.2a), thus with wave-vector parallel to the optic axis. When no electric ﬁeld is applied, the plate is isotropic for the incident ray. The electro-optical tensor rijk for point group ¯42m has the form given below in Equation (19.5) if axis Ox3 is chosen parallel to the ¯4 axis and axes Ox1 and Ox2 are parallel to the 2-fold axes. The latter are parallel to basis vectors a and b because the space group of KDP is I¯42d (Sect. 7.4). Suppose we apply an electric ﬁeld, with norm E, parallel to the optic axis, i.e. to the ¯4 axis. Tensor Δηα is such that: ⎞ ⎛ ⎞ ⎛ ⎞ ⎛ Δη1 0 0 0 0 ⎜ Δη2 ⎟ ⎜ 0 ⎛ ⎞ ⎜ 0 ⎟ 0 0 ⎟ ⎟ ⎜ ⎟ ⎜ ⎟ ⎜ 0 ⎟ ⎜ Δη3 ⎟ ⎜ 0 ⎟ ⎜ 0 0 ⎜ ⎟=⎜ ⎟⎝ 0 ⎠ = ⎜ 0 ⎟. (19.5) ⎜ Δη4 ⎟ ⎜ r41 0 ⎟ ⎜ 0 ⎟ 0 ⎟ ⎜ ⎟ ⎜ ⎟ ⎜ E ⎝ Δη5 ⎠ ⎝ 0 r41 0 ⎠ ⎝ 0 ⎠ Δη6

0

0

r63

r63 E

414

Symmetry and Physical Properties of Crystals n + r63 En3/2

x2 b

k

n – r63 En3/2

x’2

x1 a c

x2

x’1 b

x3

O

a

x1

E

(a)

(b)

Figure 19.2: (a) Schematic representation of optical propagation in a crystal of KDP submitted to an electric ﬁeld E parallel to basis vector c; (b) directions of the neutral lines of the plate (dotted lines) We obtain Δη6 = r63 E and all the other terms are zero. Tensor [η] is now given by: ⎞

⎛

1 r63 E ⎜ n2o ⎜ 1 ⎜ r E ⎜ 63 n2o ⎜ ⎝ 0 0

0

⎟ ⎟ 0 ⎟ ⎟ ⎟ 1 ⎠ n2e

where no and ne are respectively the ordinary and extraordinary indices of the KDP crystal without applied electric ﬁeld. Rotation of the axis system by 45◦ around the optic axis Ox3 makes the tensor diagonal: ⎞

⎛

1 + r63 E ⎜ n2o ⎜ ⎜ 0 ⎜ ⎜ ⎝ 0

0 1 − r63 E n2o 0

⎛ 1 ⎟ ⎜ n21 ⎟ ⎜ ⎜ 0 ⎟ ⎟=⎜ 0 ⎟ ⎜ 1 ⎠ ⎝ 0 n2e 0

⎞ 0 1 n22 0

0

⎟ ⎟ 0 ⎟ ⎟ ⎟ 1 ⎠ n23

where n1 , n2 and n3 are the principal indices. The index ellipsoid is no more an ellipsoid of revolution around Ox3 . Its principal axes are Ox3 and two axes Ox1 and Ox2 at 45◦ to the axes Ox1 and Ox2 . Ox1 and Ox2 are thus parallel to the mirrors in the crystal. We have: 1 1 = 2 + r63 E no n21

and

1 1 = 2 − r63 E no n22

Chapter 19 – Electro-optical and elasto-optical eﬀects

415

whence we deduce as above, setting Δn = n2 − n1 :

Δn 1 = −2 3 = −2r63 E, Δ n2 no Δn = n2 − n1 = n3o r63 E.

(19.6)

The neutral lines of the plate are at 45◦ to axes a and b (Fig. 19.2b).

19.2.2. Applications of the linear electro-optical eﬀect Phase-shifting plates with variable delay In the two special cases we discussed previously, applying an electric ﬁeld normal to the plate changes isotropic propagation into anisotropic propagation. The neutral lines of the plate are at 45◦ to the vectors a and b parallel to the plane of the plate. The diﬀerence between the indices for waves with polarization parallel to these neutral lines is proportional to the amplitude E of the electric ﬁeld and to an electro-optical coeﬃcient r (r14 for NaBrO3 and r63 for KDP): Δn = n3 rE. If the beam traverses a thickness e of crystal, the components of the electric ﬁeld of the wave, parallel to the neutral lines of the plate, feature, when leaving the plate, a phase diﬀerence ϕ: ϕ = 2π

n3 rEe n3 rV (Δn)e = 2π = 2π λ λ λ

(19.7)

where V is the voltage applied between the two faces of the crystal. The half-wave voltage Vπ is deﬁned as the voltage which must be applied to the crystal for the phase shift to be equal to π. It is obtained from Equation (19.6), yielding: λ (19.8) Vπ = 3 . 2n r The phase shift can then be written as: ϕ=

πV . Vπ

For a crystal of KDP, r = r63 = 10.3 pm V−1 , n = 1.51 for λ = 545 nm and Vπ = 7.8 kV. For a crystal of NaClO3 , the half-wave voltage, for the same wavelength, is equal to 200 kV. The same plates become quarter-wave plates (ϕ = π/2) if they are submitted to a voltage equal to half the half-wave voltage. We note that the value of the phase shift does not depend on the crystal thickness, but on the voltage applied between its two faces. Thus, in principle, thin crystals can be used. However, since the voltages are rather large, the crystal must be thick enough to avoid electrical breakdown.

416

Symmetry and Physical Properties of Crystals

Longitudinal ﬁeld intensity modulator Consider a crystal of KDP cut into a rectangle parallelepiped with sides parallel to the basis vectors a, b and c of the unit cell (Fig. 19.3). We choose an orthonormal coordinate system (Ox1 x2 x3 ) (the unit vectors on these axes are written as i, j and k) parallel to the basis vectors, and an axis system (Ox1 x2 x3 ) (with unit vectors i , j and k) rotated with respect to the ﬁrst one by 45◦ around Ox3 . A

x2 x1 a P

b c

x3

x2 x’2

x’1 j’

j O

i’ i

x1

L V

Figure 19.3: Intensity modulator with longitudinal ﬁeld We send onto this crystal a plane wave, with wave-vector ko parallel to Ox3 , linearly polarized along Ox2 thanks to a polarizer P. The crystal has length L along the propagation direction. Using transparent electrodes deposited on the entrance and exit surfaces of the crystal, we apply a voltage V , which creates in the crystal an electric ﬁeld E = V /L perpendicular to the plate. The electric ﬁeld of the wave incident on the entrance face of the crystal has form E0 (exp −iωt)j, the origin of the axes being chosen on the entrance face of the crystal. We saw (Sect. 19.2.1) that the neutral lines of the crystal are parallel to Ox1 and Ox2 . The incident polarization √ splits into two components parallel to the √ neutral lines (( 2/2) E0 i and ( 2/2) E0 j ), which propagate with diﬀerent indices and thus shift their phase as propagation proceeds. At the crystal exit, the electric ﬁeld of the wave can be written: √ √ 2 2 E = E0 exp i(k0 n1 L − ωt) i + E0 exp i(k0 n2 L − ωt) j (19.9) 2 2 with

n1 = no −

n3o r63 E , 2

n2 = no +

We set

k0 (n2 − n1 )L = 2δ =

so that

δ=

n3o r63 E 2

and

2π 3 2π 3 n r63 EL = n r63 V λ o λ o

π 3 n r63 V λ o

which only depends on the voltage V applied to the crystal.

k0 =

2π . λ

Chapter 19 – Electro-optical and elasto-optical eﬀects Equation (19.8) can be written as: √ 2 exp i(k0 n1 L − ωt)(i + exp 2iδj ), E = E0 2

417

(19.10)

and, in Jones notation, the electric ﬁeld has expression, in base {i , j }: " # √ 2 E 0 2 √ . E0 22 exp 2iδ We see that, depending on the value 2δ of the phase shift between the two components, the wave can take on, at the crystal exit, any polarization (see Sect. 17.1.3). The crystal is a half-wave plate if the applied voltage Vπ is such that 2δ = π, hence Vπ = λ/2n3 r63 , a value we already found in (19.7). We can thus write that 2δ = πV /Vπ . The electric ﬁeld (19.9) can also be written, to within a phase factor: √ 2 −iδ [E i + E iδ j ]. E = E0 2 A linear analyzer A, with polarization axis parallel to Ox1 , is placed after the crystal (Fig. 19.3). The crystal is thus set between crossed polarizers. The electric ﬁeld after the analyzer is the√sum of the projections onto Ox√ 1 of E. The projection of vector i is vector ( 2/2)i and that of vector j is −( 2/2)i. We obtain an electric ﬁeld E such that E0 −iδ E = − E iδ ]i [E 2 = −iE0 sin δ i. The transmitted intensity I is proportional to the square of the amplitude of the electric ﬁeld (Sect. 16.3), so that:

π V I = I0 sin2 δ = I0 sin2 2Vπ where we note I0 the intensity incident on the crystal. If we apply a voltage equal to Vπ , the intensity is maximum and equal to the intensity transmitted by the polarizer, whereas at zero voltage the intensity is zero (isotropic propagation, crystal placed between crossed polarizer and analyzer). This device can then be used as a beam switch, by changing from voltage Vπ (I = I0 ) to zero voltage (I = 0). If a DC voltage equal to Vπ /2 is sinusoidally modulated with amplitude much smaller than Vπ , the intensity of the light beam is modulated quasi-sinusoidally. The slope of the function I(V ) is nearly constant in the vicinity of Vπ /2 (Fig. 19.4), so that the relation between the voltage variation and the variation in transmitted intensity is quasi-linear. In this setup, the voltage Vπ does not depend on the crystal length; it can therefore not be optimized. Also it is not easy to make transparent electrodes. The setup described next, with transverse ﬁeld, is therefore preferred.

418

Symmetry and Physical Properties of Crystals I/I0 1

V(t)/V

I(t)/I0

0

V/V

1

Figure 19.4: Analog modulation, using the experimental device schematically shown on Figure 19.3 Transverse ﬁeld intensity modulator The crystal used is again a rectangle parallelepiped of KDP, but cut so that its sides are parallel to Ox3 , Ox1 and Ox2 , with the incident beam parallel to Ox1 (Fig. 19.5). It is placed between crossed polarizer and analyzer, the polarization direction of the analyzer being at an angle of 45◦ to the sides of the entrance face of the crystal. The electric ﬁeld is parallel to Ox3 . A

x3 x’2 P

c

b

x’1

a

45°

x3

45°

n

V

k O

L

m j’

x’2

Figure 19.5: Intensity modulator with transverse ﬁeld The neutral lines of the plate are Ox3 and Ox2 , and only the index for the component parallel to Ox2 is modulated by the electric ﬁeld. We note that, in the absence of the electric ﬁeld, the crystal is birefringent for the chosen propagation direction. On the entrance face of the plate, the electric ﬁeld of the light wave can be written as: √ 2 (j + k) exp(− iωt) E = E0 2 taking the origin on the entrance face of the crystal.

Chapter 19 – Electro-optical and elasto-optical eﬀects

419

After the plate, the electric ﬁeld becomes: √

2 1 3 j exp ik0 L no + no r63 E + k exp ik0 Lne exp(−iωt). E = E0 2 2 We set:

1 k0 L(ne − no − n3o r63 E) = 2δ 2 and the electric ﬁeld becomes: √

1 3 2 exp ik0 L no + no r63 E [j + exp 2iδ k] exp(−iωt) E = E0 2 2 and, in Jones notation in base {j , k} : " # " # √ √ 2 2 E E exp −iδ 0 0 2 2√ √ or . E0 22 exp 2iδ E0 22 exp iδ We can thus write the electric ﬁeld, to within a phase factor: √ 2 E = E0 (exp −i δ j + exp i δ k). 2 After the analyzer, the electric ﬁeld E is the projection of E on the unit vector n parallel to the analyzer (Fig. 19.5): E =

E0 [− exp −iδ + exp iδ]n = i(E0 sin δ)n 2

and the intensity I of the light beam is:

1 V πL ne − no − n3o r63 I = I0 sin2 δ = I0 sin2 λ 2 where is the thickness of the crystal in the direction of Ox3 and V the applied voltage (E = V /). We see that the voltage Vπ which changes the phase shift 2δ by π can be strongly decreased if the crystal specimen is long and thin, since: λ . Vπ = 3 no r63 L The disadvantage of this conﬁguration is the strong birefringence, which induces a very large phase shift in the absence of an applied electric ﬁeld. This birefringence is temperature-sensitive, and the operating point is unstable. To minimize this eﬀect, two identical crystals, rotated by 90◦ around Ox1 , are placed one after the other, so as to cancel the total birefringence. The two crystals must then be submitted to opposite voltages, so that the electrooptical eﬀects add (Exercise 19.1). The two crystals are placed in a thermally insulated box so that they are at the same temperature.

420

Symmetry and Physical Properties of Crystals

19.2.3. Quadratic electro-optical eﬀect, or Kerr eﬀect General properties This eﬀect is much weaker than the linear eﬀect. Therefore, it shows up appreciably only when the linear eﬀect is zero, i.e. in centrosymmetric crystals and in liquids. It is deﬁned by the following relation: ηij (E) − ηij (E = 0) = Δηij = zijkl Ek El where the zijkl are the components of the rank-4 electro-optical tensor, the Kerr tensor [z]. Δηij is symmetric and Ek and El can be interchanged. The matrix of coeﬃcients zijkl can therefore be contracted. The transformation from zijkl to zαβ is performed by writing: ⎛ ⎞ ⎛ ⎞⎛ ⎞ Δη1 z11 z12 z13 z14 z15 z16 E12 ⎜ Δη2 ⎟ ⎜ z21 z22 z23 z24 z25 z26 ⎟ ⎜ E22 ⎟ ⎜ ⎟ ⎜ ⎟⎜ ⎟ ⎜ Δη3 ⎟ ⎜ z31 z32 z33 z34 z35 z36 ⎟ ⎜ E32 ⎟ ⎜ ⎟=⎜ ⎟⎜ ⎟ ⎜ Δη4 ⎟ ⎜ z41 z42 z43 z44 z45 z46 ⎟ ⎜ 2E2 E3 ⎟ . ⎜ ⎟ ⎜ ⎟⎜ ⎟ ⎝ Δη5 ⎠ ⎝ z51 z52 z53 z54 z55 z56 ⎠ ⎝ 2E3 E1 ⎠ Δη6 z61 z62 z63 z64 z65 z66 2E1 E2 Thus zαβ = zijkl whatever α and β, as in the case of the stiﬀness tensor. However, in contrast to the tensors of elasticity, the quadratic electro-optical tensor [z] has no reason to be symmetric with respect to α and β, because no thermodynamic argument can be invoked. Thus, for a triclinic crystal (point groups 1 and ¯1), the 36 coeﬃcients are independent. Tables 19.2a and 19.2b show the various non-zero terms of the tensor as a function of the crystal symmetry. The coeﬃcients of this tensor are expressed in m2 V−2 and are on the order of 10−18 . Application to isotropic materials Most applications of the Kerr electro-optical eﬀect concern isotropic materials such as liquids. To know the form of the tensor, we start out from the tensor for the most symmetrical cubic materials (group m¯3m) and then show, as was done for the stiﬀness coeﬃcients (Sect. 13.6), that the three coeﬃcients z11 , z12 and z44 are connected through relation: 1 z44 = (z11 − z12 ). 2 Suppose we apply an electric ﬁeld E. The form of tensor zαβ is independent of the choice of axes, since the material is isotropic. We can therefore choose the axis directions to suit ourselves, for example take Ox1 parallel to the electric ﬁeld.

Chapter 19 – Electro-optical and elasto-optical eﬀects

421

Table 19.2a: Form of the matrices representing the coeﬃcients zαβ (and pαβ ) for the various point groups P.G.

Triclinic

Monoclinic

1 ¯1

2 m 2 m 2 // Ox2 2 m 2 m 2 // Ox3

Orthorhombic

222 mm2 mmm ⎛

Tetragonal

4 ¯4 4 m

422 4mm ¯42m 4 mm m

⎛ z11 ⎜z21 ⎜ ⎜z31 ⎜ ⎜z41 ⎜ ⎝z51 z61 ⎛ z11 ⎜z21 ⎜ ⎜z31 ⎜ ⎜0 ⎜ ⎝z51 0 ⎛ z11 ⎜z21 ⎜ ⎜z31 ⎜ ⎜0 ⎜ ⎝0 z61 ⎛ z11 ⎜z21 ⎜ ⎜z31 ⎜ ⎜0 ⎜ ⎝0 0

zαβ z12 z22 z32 z42 z52 z62

z13 z23 z33 z43 z53 z63

z14 z24 z34 z44 z54 z64

z12 z22 z32 0 z52 0

z13 0 z23 0 z33 0 0 z44 z53 0 0 z64

z12 z22 z32 0 0 z62

z13 0 z23 0 z33 0 0 z44 0 z54 z63 0

z12 z13 0 z22 z23 0 z32 z33 0 0 0 z44 0 0 0 0 0 0

z11 z12 ⎜z12 z11 ⎜ ⎜z31 z31 ⎜ ⎜ 0 0 ⎜ ⎝ 0 0 z61 −z 61 ⎛ z11 z12 ⎜z12 z11 ⎜ ⎜z31 z31 ⎜ ⎜0 0 ⎜ ⎝0 0 0 0

z15 z25 z35 z45 z55 z65

⎞ z16 z26 ⎟ ⎟ z36 ⎟ ⎟ z46 ⎟ ⎟ z56 ⎠ z66

⎞ z15 0 z25 0 ⎟ ⎟ z35 0 ⎟ ⎟ 0 z46 ⎟ ⎟ z55 0 ⎠ 0 z66 ⎞ 0 z16 0 z26 ⎟ ⎟ 0 z36 ⎟ ⎟ z45 0 ⎟ ⎟ z55 0 ⎠ 0 z66 ⎞ 0 0 0 0⎟ ⎟ 0 0⎟ ⎟ 0 0⎟ ⎟ z55 0 ⎠ 0

z66

⎞ z13 0 0 z16 z13 0 0 −z 16 ⎟ ⎟ z33 0 0 0 ⎟ ⎟ 0 ⎟ 0 z44 z45 ⎟ 0 ⎠ 0 −z 45 z44 0 0 0 z66 ⎞ z13 0 0 0 z13 0 0 0⎟ ⎟ z33 0 0 0⎟ ⎟ 0⎟ 0 z44 0 ⎟ 0 0 z44 0 ⎠ 0 0 0 z66

422

Symmetry and Physical Properties of Crystals Table 19.2b: Form of the matrices representing the coeﬃcients zαβ (and pαβ ) for the various point groups (continued); z ∗ = 12 (z11 − z12 ) P.G.

Rhomboedral

3 ¯3

32 3m ¯3m

Hexagonal

6 ¯6 6 m 622 6mm ¯62m 6 mm m

Cubic

23 m¯3

432 ¯43m m¯3m

Isotropic

⎛

zαβ

⎞ z11 z12 z13 z14 z15 z16 ⎜ z12 z11 z13 −z 14 −z 15 −z 16 ⎟ ⎜ ⎟ z31 z33 0 0 0 ⎟ ⎜ z31 ⎜ ⎟ z44 z45 −z 51 ⎟ ⎜ z41 −z 41 0 ⎝ z −z 51 0 −z 45 z44 z41 ⎠ 51 −z 16 z16 0 −z 15 z14 z∗ ⎛ ⎞ 0 0 z11 z12 z13 z14 0⎟ ⎜z12 z11 z13 −z 14 0 ⎜ ⎟ 0 0 0⎟ ⎜z31 z31 z33 ⎜ ⎟ z44 0 0⎟ ⎜z41 −z41 0 ⎝0 0 0 0 z44 z41 ⎠ 0 0 0 0 z14 z ∗ ⎛ ⎞ 0 0 z16 z11 z12 z13 0 0 −z 16 ⎟ ⎜ z12 z11 z13 ⎜ ⎟ 0 0 0 ⎟ ⎜ z31 z31 z33 ⎜ ⎟ 0 ⎟ 0 0 z44 z45 ⎜ 0 ⎝ 0 0 ⎠ 0 0 −z 45 z44 0 0 z∗ −z 16 z16 0 ⎛ ⎞ 0 0 z11 z12 z13 0 ⎜z12 z11 z13 0 0 0⎟ ⎜ ⎟ 0 0⎟ ⎜z31 z31 z33 0 ⎜ ⎟ 0⎟ 0 0 z44 0 ⎜ 0 ⎝ 0 0 0 0 z44 0 ⎠ 0 0 0 0 0 z∗ ⎛ ⎞ 0 0 z11 z12 z21 0 ⎜z21 z11 z12 0 0 0⎟ ⎜ ⎟ 0 0⎟ ⎜z12 z21 z11 0 ⎜ ⎟ 0⎟ 0 0 z44 0 ⎜0 ⎝0 0 0 0 z44 0 ⎠ 0 0 0 0 0 z44 ⎛ ⎞ 0 0 z11 z12 z12 0 0 0⎟ ⎜z12 z11 z12 0 ⎜ ⎟ 0 0⎟ ⎜z12 z12 z11 0 ⎜ ⎟ 0⎟ 0 0 z44 0 ⎜0 ⎝0 0 0 0 z44 0 ⎠ 0 0 0 0 0 z44 ⎛ ⎞ z11 z12 z12 0 0 0 ⎜z12 z11 z12 0 0 0 ⎟ ⎜ ⎟ ⎜z12 z12 z11 0 0 0 ⎟ ⎜ ⎟ 0 0 z∗ 0 0 ⎟ ⎜0 ⎝0 ∗ 0⎠ 0 0 0 z 0 0 0 0 0 z∗

Chapter 19 – Electro-optical and elasto-optical eﬀects Tensor [Δη] becomes: ⎞ ⎛ ⎛ Δη1 z11 z12 z12 ⎜ Δη2 ⎟ ⎜ z12 z11 z12 ⎟ ⎜ ⎜ ⎜ Δη3 ⎟ ⎜ z12 z12 z11 ⎜ ⎟ ⎜ ⎜ Δη4 ⎟ = ⎜ z44 ⎜ ⎟ ⎜ ⎝ Δη5 ⎠ ⎝ z44 Δη6 z44 and we obtain for tensor [η]: ⎛ 1 2 ⎜ n2 + z11 E ⎜ ⎜ 0 ⎜ ⎝ 0

⎞⎛ ⎟⎜ ⎟⎜ ⎟⎜ ⎟⎜ ⎟⎜ ⎟⎜ ⎠⎝

423

E2 0 0 0 0 0

⎞

⎛

⎟ ⎜ ⎟ ⎜ ⎟ ⎜ ⎟=⎜ ⎟ ⎜ ⎟ ⎜ ⎠ ⎝

z11 E 2 z12 E 2 z12 E 2 0 0 0

⎞ ⎟ ⎟ ⎟ ⎟ ⎟ ⎟ ⎠

⎞ 0

0

1 + z12 E 2 n2 0

0 1 + z12 E 2 n2

⎟ ⎟ ⎟ ⎟ ⎠

where n is the optical index of the liquid. The material is no more isotropic: it has become uniaxial, with the optic axis parallel to the applied electric ﬁeld, and with ordinary index no and extraordinary index ne calculated as in (19.4) since the index change is very small: no = n − n3 z12

E2 2

and

ne = n − n3 z11

E2 . 2

The index ellipsoid is of revolution around the direction of the electric ﬁeld. A Kerr cell contains a liquid to which an electric ﬁeld E is applied normal to the propagation direction of the incident wave (Fig. 19.6a). Two waves propagate in the liquid, one with polarization parallel to E with index ne , the other with index no (Fig. 19.6b). The diﬀerence Δn between the indices is given by: Δn = ne − no = n3 (z12 − z11 ) or

Δn = −n3 z44 E 2 ,

E2 2

(19.11)

which is often written as: ne − no = KλE 2 by setting K=

n3 z44 n3 (z12 − z11 ) =− . 2λ λ

(19.12)

(19.13)

K is the Kerr constant. If the material were not isotropic, but had point group 432 or m¯3 or m¯3m (cubic groups for which the linear electro-optical eﬀect is zero), we would obtain the same result provided the electric ﬁeld is applied parallel to one of the basis vector of the unit cell. The Kerr constant is equal to n3 (z12 − z11 )/2λ (and is no more equal to −n3 z44 /λ).

424

Symmetry and Physical Properties of Crystals x1 + De E

Do

k

x3

x2 –

(a)

(b)

Figure 19.6: (a) Schematic representation of the principle of a Kerr cell; (b) construction of the polarization vectors using the index ellipsoid

19.3. Elasto-optical eﬀects 19.3.1. Deﬁnition Applying stress (tensor [T ]) or a strain (tensor [S]) can lead to a variation [Δη] of the electrical impermeability tensor [η], expressed to ﬁrst order by: Δηij = pijkl Skl , Δηij = πijkl Tkl . The coeﬃcients pijkl and πijkl are those of rank-4 tensors (called elasto-optical tensor and piezo-optical tensor respectively), since each of them connects a rank-2 tensor (the strain tensor [S] or the stress tensor [T ]) to another rank-2 tensor (tensor [Δη]). Tensors [S], [T ] and [Δη] are symmetric. We can therefore contract the coeﬃcients pijkl and πijkl , as was done previously for the elastic tensors and for the Kerr eﬀect tensor. The transformation rules for going from the Sij to the Sα and from the Tij to the Tα make it clear that:

and

pαβ = pijkl παβ = πijkl παβ = 2πijkl

for all α and β for α = 1 to 6 and β = 1 to 3 for α = 1 to 6 and β = 4 to 6.

Matrices pαβ and παβ have no reason to be symmetric with respect to α and β since no thermodynamic argument can be invoked. The eﬀect of crystal symmetry on the number of independent coeﬃcients in tensor [p] is determined in the same way as for the Kerr eﬀect tensor [z]. Table 19.2a and 19.2b are therefore valid for tensor [p] too. The table of independent coeﬃcients for tensor [π] is slightly diﬀerent (Tab. 19.3a and 19.3b) because contraction is not performed the same way.

Chapter 19 – Electro-optical and elasto-optical eﬀects

425

Table 19.3a: Form of the matrices representing coeﬃcients παβ for the various point groups P.G.

Triclinic

1 ¯1

Monoclinic

2 m 2 m 2 // Ox2 2 m 2 m 2 // Ox3

Orthorhombic

Tetragonal

222 mm2 mmm

4 ¯4 4 m

422 4mm ¯42m 4 mm m

⎛

π11 ⎜π21 ⎜ ⎜π31 ⎜ ⎜π41 ⎜ ⎝π51 π61 ⎛ π11 ⎜π21 ⎜ ⎜π31 ⎜ ⎜ 0 ⎜ ⎝π51 0 ⎛ π11 ⎜π21 ⎜ ⎜π31 ⎜ ⎜ 0 ⎜ ⎝ 0 π61 ⎛ π11 ⎜π21 ⎜ ⎜π31 ⎜ ⎜ 0 ⎜ ⎝ 0 0

παβ

⎞ π16 π26 ⎟ ⎟ π36 ⎟ ⎟ π46 ⎟ ⎟ π56 ⎠ π66 ⎞ 0 0 ⎟ ⎟ 0 ⎟ ⎟ π46 ⎟ ⎟ 0 ⎠ π66 ⎞ π16 π26 ⎟ ⎟ π36 ⎟ ⎟ 0 ⎟ ⎟ 0 ⎠

π12 π22 π32 π42 π52 π62

π13 π23 π33 π43 π53 π63

π14 π24 π34 π44 π54 π64

π15 π25 π35 π45 π55 π65

π12 π22 π32 0 π52 0

π13 0 π23 0 π33 0 0 π44 π53 0 0 π64

π15 π25 π35 0 π55 0

π12 π22 π32 0 0 π62

π13 0 0 π23 0 0 π33 0 0 0 π44 π45 0 π54 π55 π63 0 0 π66

⎞ π12 π13 0 0 0 π22 π23 0 0 0 ⎟ ⎟ π32 π33 0 0 0 ⎟ ⎟ 0 ⎟ 0 0 π44 0 ⎟ 0 0 0 π55 0 ⎠ 0 0 0 0 π66

⎛ π11 π12 ⎜π12 π11 ⎜ ⎜π31 π31 ⎜ ⎜ 0 0 ⎜ ⎝ 0 0 π61 −π61 ⎛ π11 π12 ⎜π12 π11 ⎜ ⎜π31 π31 ⎜ ⎜ 0 0 ⎜ ⎝ 0 0 0 0

⎞ π13 0 0 π16 π13 0 0 −π16 ⎟ ⎟ π33 0 0 0 ⎟ ⎟ 0 ⎟ 0 π44 π45 ⎟ 0 ⎠ 0 −π45 π44 0 0 0 π66 ⎞ π13 0 0 0 π13 0 0 0 ⎟ ⎟ π33 0 0 0 ⎟ ⎟ 0 ⎟ 0 π44 0 ⎟ 0 0 π44 0 ⎠ 0 0 0 π66

426

Symmetry and Physical Properties of Crystals Table 19.3b: Form of the matrices representing coeﬃcients παβ for the various point groups (continued); π ∗ = (π11 − π12 ) P.G.

Rhombohedral

3 ¯3

32 3m ¯3m

Hexagonal

6 ¯6 6 m 622 6mm ¯62m 6 mm m

Cubic

23 m¯3

432 ¯43m m¯3m

Isotropic

⎛

παβ

⎞ π15 −2π61 π11 π12 π13 π14 ⎜π12 π11 π13 −π14 −π15 2π61 ⎟ ⎜ ⎟ ⎜π31 π31 π33 0 0 0 ⎟ ⎜ ⎟ ⎜π41 −π41 0 π44 π45 −2π51 ⎟ ⎜ ⎟ ⎝π51 −π51 0 −π45 π44 2π41 ⎠ π61 −π61 0 −π15 π14 π∗ ⎛ ⎞ 0 0 π11 π12 π13 π14 ⎜π12 π11 π13 −π14 0 0 ⎟ ⎜ ⎟ ⎜π31 π31 π33 ⎟ 0 0 0 ⎜ ⎟ ⎜π41 −π41 0 ⎟ π 0 0 44 ⎜ ⎟ ⎝ 0 0 0 0 π44 2π41 ⎠ 0 0 0 0 π14 π ∗ ⎛ ⎞ π11 π12 π13 0 0 −2π61 ⎜π12 π11 π13 0 0 2π61 ⎟ ⎜ ⎟ ⎜π31 π31 π33 0 0 0 ⎟ ⎜ ⎟ ⎜ 0 0 ⎟ 0 0 π44 π45 ⎜ ⎟ ⎝ 0 0 ⎠ 0 0 −π45 π44 0 0 π∗ π61 −π61 0 ⎛ ⎞ 0 0 π11 π12 π13 0 ⎜π12 π11 π13 0 0 0⎟ ⎜ ⎟ ⎜π31 π31 π33 0 0 0⎟ ⎜ ⎟ ⎜ 0 0⎟ 0 0 π44 0 ⎜ ⎟ ⎝ 0 0 0 0 π44 0 ⎠ 0 0 0 0 0 π∗ ⎛ ⎞ 0 0 π11 π12 π13 0 ⎜π13 π11 π12 0 0 0 ⎟ ⎜ ⎟ ⎜π12 π13 π11 0 0 0 ⎟ ⎜ ⎟ ⎜ 0 0 ⎟ 0 0 π44 0 ⎜ ⎟ ⎝ 0 0 0 0 π44 0 ⎠ 0 0 0 0 0 π44 ⎛ ⎞ 0 0 π11 π12 π12 0 ⎜π12 π11 π12 0 0 0 ⎟ ⎜ ⎟ ⎜π12 π12 π11 0 0 0 ⎟ ⎜ ⎟ ⎜ 0 0 ⎟ 0 0 π44 0 ⎜ ⎟ ⎝ 0 0 0 0 π44 0 ⎠ 0 0 0 0 0 π44 ⎛ ⎞ π11 π12 π12 0 0 0 ⎜π12 π11 π12 0 0 0 ⎟ ⎜ ⎟ ⎜π12 π12 π11 0 0 0 ⎟ ⎜ ⎟ ⎜ 0 0 0 π∗ 0 0 ⎟ ⎜ ⎟ ⎝ 0 0 0 0 π∗ 0 ⎠ 0 0 0 0 0 π∗

Chapter 19 – Electro-optical and elasto-optical eﬀects

427

Tensors [p] and [π] are mutually related, since tensors [S] and [T ] are: [S] = [s][T ] and [T ] = [c][S], hence: pijkl = πijmn cmnkl

and

πijkl = pijmn smnkl .

The coeﬃcients pijkl are dimensionless since [S] and [Δη] are, and their maximum value is of the order of 1 (and usually closer to 0.1). The coeﬃcients πijkl are dimensionally reciprocal stresses, and are of the order of 10−12 m2 N−1 . The variation in refractive index, under the eﬀect of stress, is used to analogically evidence stresses in mechanical parts, normally metallic, through the use of models made of transparent and isotropic plastics such as acrylics (Plexiglas , Lucite , Perspex , Altuglas ).

19.3.2. Application to the acousto-optical eﬀects An acoustic wave is a strain wave. In photo-elastic crystals, i.e. those featuring elasto-optical eﬀects, the acoustic wave gives rise to variations in index which it may be of interest to create at will. Consider for example a crystal of lead molybdate, PbMoO4 , with point group 4/m. It is uniaxial, with optical axis parallel to the 4-fold axis. Suppose we excite in this crystal a longitudinal acoustic wave with wave-vector K parallel to the 4-fold axis. This wave creates a displacement u parallel to the 4-fold axis. We choose an orthonormal coordinate system with Ox3 parallel to this 4-fold axis. The longitudinal displacement then has only one component u3 : u3 = a sin(Kx3 − Ωt) where Ω is the angular frequency of the acoustic wave. This displacement induces a strain tensor which has only one non-zero term: S3 =

∂u3 = aK cos(Kx3 − Ωt) = S0 cos(Kx3 − Ωt), ∂x3

where we set, to simplify the expression, S0 = aK. The strain induces a variation in the impermeability tensor given by: ⎞ ⎛ ⎞⎛ ⎞ ⎛ ⎛ p11 0 p12 p13 p16 Δη1 p13 S3 ⎟ ⎜ ⎟ ⎜ Δη2 ⎟ ⎜ p12 ⎜ p p −p p 0 11 13 16 ⎟⎜ ⎟ ⎜ ⎟ ⎜ 13 S3 ⎜ ⎟ ⎜ ⎜ Δη3 ⎟ ⎜ p31 ⎟ ⎜ p p S 31 33 ⎟ ⎜ ⎟⎜ 3 ⎟ = ⎜ p33 S3 ⎜ ⎟ ⎜ ⎜ Δη4 ⎟ = ⎜ ⎟ ⎜ 0 p p 0 44 45 ⎟ ⎜ ⎟⎜ ⎜ ⎟ ⎜ ⎠⎝ 0 ⎠ ⎝ 0 ⎝ Δη5 ⎠ ⎝ −p45 p44 Δη6 p61 −p61 p66 0 0

⎞ ⎟ ⎟ ⎟ ⎟. ⎟ ⎟ ⎠

428

Symmetry and Physical Properties of Crystals

The crystal, when no acoustic wave is excited, has principal indices n1 = n2 = no and n3 = ne , where no and ne are the ordinary and extraordinary indices respectively. With the acoustic wave, tensor [η] becomes: ⎞ ⎛ 1 + p S 0 0 13 3 ⎟ ⎜ n2o ⎟ ⎜ 1 ⎟ ⎜ 0 + p S 0 ⎟. ⎜ 13 3 n2o ⎟ ⎜ ⎠ ⎝ 1 0 0 + p33 S3 . 2 ne The crystal remains uniaxial, with its optic axis parallel to Ox3 , but its ordinary and extraordinary indices have changed to become no and ne respectively. We obtain: 1 1 = 2 + p13 S3 no no2

and

1 1 = 2 + p33 S3 . ne ne2

1 no = no − n3o p13 S0 cos(Kx3 − Ωt), 2 1 3 ne = ne − ne p33 S0 cos(Kx3 − Ωt). 2

Thus

The acoustic wave creates, within the crystal, a modulation of the ordinary and extraordinary indices, periodic along Ox3 , i.e. a grating with period Λ = 2π/K (Fig. 19.7a). The propagation velocity of this index modulation is that of the acoustic wave (V = Ω/K), on the order of a few km s−1 , which is extremely small compared to the propagation velocity of light. During the time it takes light to propagate through the crystal, the grating can therefore be considered as motionless. K

K

E k

x2

O

c

x1

x1 x3

x3

(a)

(b)

Figure 19.7: (a) Schematic representation of diﬀraction of a wave by a crystal of PbMoO4 excited by an acoustic wave with wave-vector K; (b) Bragg diﬀraction on the acoustic grating

Chapter 19 – Electro-optical and elasto-optical eﬀects

429

Suppose we send onto this crystal an optical wave with wave-vector k belonging to plane (Ox1 , Ox3 ), linearly polarized along Ox2 . This wave propagates in the crystal with the index no , modulated by the acoustic wave. It is diﬀracted by this refractive index grating, in the same way as an X-ray wave is diﬀracted by a crystal. The diﬀraction condition for a wave incident on the crystal at an angle θ with the lattice planes can be expressed, as for Bragg “reﬂection” (diﬀraction) (see Sect. 3.2.3), by: 2Λ sin θ = λ/no .

(19.14)

The refractive index does not show up in the expression for X-ray diﬀraction because it is then practically equal to 1. Therefore, the beam is, after diﬀraction, deviated by an angle 2θ when the acoustic wave is excited (Fig. 19.7b). The device is an optical deﬂector. The value of theta is on the order of a degree, as shown by the calculation below. For a crystal of PbMoO4 and an optical wavelength of 500 nm in air, the ordinary index is 2.3. If the acoustic wave has frequency 500 MHz, its propagation velocity in the crystal is 3750 m s−1 . Its wavelength is 7.5 μm. The diﬀraction condition becomes sin θ = 0.0145 and θ = 0.83◦ , so that the deviation of the beam is 1.67◦ . We assumed, as a ﬁrst approximation, that the index grating created by the acoustic wave is ﬁxed. Actually, its motion leads, via the Doppler eﬀect, to a (very small) variation Δω of the diﬀracted wave frequency. This variation is given by: 2V// Δω = ω (c/n) where V// is the projection of the acoustic wave velocity V onto the propagation direction of the optical wave. If the acoustic wave propagates toward the optical wave (as on Fig. 19.7b), Δω is positive, while it is negative in the opposite case. Here V// = V sin θ, and Δω 2V sin θ = . ω (c/n) Taking into account (19.13) and ω = 2πc/λ, Δω =

2πV = Ω. Λ

The diﬀracted wave has an angular frequency ω slightly diﬀerent from ω. ω = ω ± Ω. The + sign corresponds to the case of Figure 19.7, while the − sign corresponds to propagation of the acoustic wave in the opposite direction.

430

Symmetry and Physical Properties of Crystals

This result can be interpreted in terms of particles. An electromagnetic wave with angular frequency ω and wave-vector k is a ﬂow of photons with energy ω and momentum k. The acoustic wave with angular frequency Ω and wavevector K is a set of phonons with energy Ω and momentum K. Diﬀraction of light by the acoustic wave can be viewed as a collision between particles. In the case of Figure 19.7, an incident photon (ω, k) and a phonon (Ω, K) disappear while a new photon (ω , k ) is created. Conservation of energy and of momentum imply: ω = ω + Ω k = k + K. If the acoustic wave were propagating the other way, an incident photon (ω, k) would disappear and a phonon (Ω, K) and a diﬀracted photon (ω , k ) would be created, with ω = ω − Ω k = k − K.

19.4. Exercises Electro-optical eﬀect Exercise 19.1. A block of LiNbO3 (point group 3m) has the shape of a rectangle parallelepiped. Its entrance face is parallel to one of the mirrors and one of the sides of this face is parallel to the 3-fold axis (coinciding with the optic axis). We choose an orthonormal axis set such that Ox3 is parallel to the optic axis and Ox1 is perpendicular to the entrance face. An electric ﬁeld, parallel to Ox3 and pointing toward the positive Ox3 direction, is applied via transparent electrodes deposited on the faces perpendicular to Ox3 (see ﬁgure below).

c O7

x3

x1

E

1.

Show that the crystal remains uniaxial.

2.

A beam of light, perpendicular to the plate and polarized linearly, is sent onto this crystal. Calculate the phase shift ϕ between the components parallel to Ox2 and Ox3 of the electric ﬁeld of the wave, the thickness of crystal traversed being e.

Chapter 19 – Electro-optical and elasto-optical eﬀects 3.

431

After the ﬁrst crystal there is a second crystal, identical to the ﬁrst one (including for the position of the electrodes). It is rotated, with respect to the ﬁrst one, by 90◦ around the propagation direction. It is submitted to an electric ﬁeld with the same norm as that applied to the ﬁrst crystal, but with inverse polarity. Calculate the phase shift ϕ which will add to the phase shift ϕ between the same components of the incident wave. Calculate the thickness e of each crystal so that the total phase shift is equal to π. Numerically: E = 500 V cm−1 ; λ = 633 nm and no = 2.200; ne = 2.286; r13 = 9.6 × 10−12 m V−1 ; r33 = 30.9 × 10−12 m V−1 .

Exercise 19.2 CdTe is a cubic crystal with point group ¯43m. In a system of orthonormal axes parallel to the basis vectors a, b and c, the electro-optical tensor has three nonzero coeﬃcients r41 , r52 and r63 . They are equal: r41 = r52 = r63 = r. For CdTe, r = 4.5 × 10−12 m V−1 . The index n of CdTe for λ = 1 μm is 2.84. An electric ﬁeld E is applied in the [111] direction. 1.

Show that, under this electric ﬁeld, the crystal becomes uniaxial. Determine the direction of the optic axis. Calculate the ordinary and extraordinary indices for E = 2 × 105 V m−1 .

2.

A crystal of CdTe is cut into a rectangle parallelepiped. One of the sides of the entrance face of the crystal is parallel to [111]. An electric ﬁeld is applied parallel to this [111] direction. A beam, with wavelength λ = 1 μm, is perpendicular to the entrance face and traverses this block over a length L = 8 cm. What is the ﬁeld required to obtain a half-wave plate?

Exercise 19.3 ¯ A crystal with point group 42m is optically uniaxial. It is submitted to an electric ﬁeld parallel to the ¯4 axis. Using the Curie principle, determine whether the crystal remains uniaxial. Consider the same question if the crystal has point group 4mm and if the electric ﬁeld is applied parallel to the 4-fold axis. Check the results using the linear electro-optical tensor for each of these point groups.

Elasto-optical eﬀect Exercise 19.4 A crystal of NaCl, with point group m¯3m, is submitted to a uniaxial stress T along direction [1¯10]. 1.

Show that the crystal becomes biaxial. With T = 2 × 108 N m−2 , n0 = 1.54423 and with π11 = 0.25, π12 = 1.46, π44 = −0.85 (in units

432

Symmetry and Physical Properties of Crystals 10−12 m2 N−1 ), calculate the values of the principal indices for this stressed crystal.

2.

The entrance face of the crystal is a (111) surface, and it is illuminated in normal incidence. What are the waves which propagate in the crystal, and what are the corresponding indices?

Exercise 19.5 For point groups 432, ¯43m, m¯3m, show that the variation in refractive index produced by a hydrostatic pressure p is given by: Δn =

n3 (π11 + 2π12 )p. 6

Show that Δn can also be written in the form Δn = (n3 /6) χ (p11 + 2p12 )p, where the pmn are the components of the elasto-optical tensor, and χ the bulk compressibility of the crystal.

Acousto-optical eﬀect Exercise 19.6 Germanium is transparent in the infra-red range, and has point group m¯3m. A transverse acoustic wave, with frequency f = 500 MHz, is excited in a crystal of germanium. The wave, with amplitude A, is polarized along [010] and propagates along direction [001] (see Sect. 14.3.1). Its propagation velocity is given by vt = c44 /ρ and its value is 3580 m s−1 in germanium. 1.

What strain does this wave produce?

2.

Determine the eﬀect on the propagation of a light wave induced by this strain, by calculating (a) the induced index variations, (b) the period of the index grating thus produced.

Chapter 19 – Electro-optical and elasto-optical eﬀects

433

Complement 19C. Frequency doubling, or Second Harmonic Generation (SHG) In this chapter, we investigated the inﬂuence of a static electric ﬁeld on the polarization of a crystal by an electromagnetic wave. This is a special case of a non-linear eﬀect connecting the polarization of a crystal to the electromagnetic ﬁeld(s) that propagate in it. Equation (19.3) can be written, neglecting the spatial dispersion term: Pi (ω) = χij Ej (ω) + χijk Ejs Ek (ω) + . . . ε0 This is a special case of a more general relation: Pi (ω3 ) = χij Ej (ω3 ) + χijk Ej (ω1 )Ek (ω2 ) + . . . ε0 which can be interpreted as follows. If two electromagnetic waves, with angular frequencies respectively ω1 and ω2 , propagate in a crystal, they entail distortions of the electric charge distribution in the crystal, which can oscillate with angular frequency ω3 , a combination of the angular frequencies ω1 and ω2 (ω3 = ω1 ± ω2 ), and thus radiate with the same angular frequency ω3 . The Pockels eﬀect (Sect. 19.2.1) corresponds to ω1 = 0, ω2 = ω and ω3 = ω1 + ω2 = ω. Second harmonic generation corresponds to ω1 = ω2 = ω and ω3 = ω1 + ω2 = 2ω. This phenomenon was evidenced by Franken, Hill, Peters and Weinreich1 in 1961. They focused the beam from a ruby laser (wavelength 694.3 nm) on a quartz crystal, and analyzed the outgoing beam with a prism. They observed, next to the beam with wavelength 694.3 nm, a beam with very low intensity, with wavelength half (347.1 nm) that of the incident beam, hence with twice the angular frequency. The second harmonic yield was then 10−8 . A schematic representation of the experiment is shown on Figure 19C.1. Because χijk is a third-rank tensor property, second harmonic generation is possible only in non-centrosymmetric crystals. Ruby laser

Focusing lens

Quartz crystal

Prism and collimating lenses

694 nm 347 nm

Figure 19C.1: Schematic representation of the setup for second harmonic generation 1. P.A. Franken et al., Generation of optical harmonics, Phys. Rev. Lett. 7 (4), 118 (1961).

434

Symmetry and Physical Properties of Crystals

Using a material more eﬃcient than quartz, a laser with higher intensity, and the phase match property discussed below makes it possible to obtain much better yields. The investigation of the form of the electric ﬁelds shows that the ratio of the powers delivered at the angular frequencies 2ω and ω respectively is proportional to the beam power, to the angular frequency ω, and to the function sin2 ΔkL 2 ΔkL 2

(19C.1)

2

where L is the length of crystal traversed and Δk = k(2ω) − 2k(ω). It is clear that the above function is maximal for Δk = 0 so that k(2ω) − 2k(ω) = 0, which means n(2ω)

ω 2ω = 2n(ω) , c c

so that n(2ω) = n(ω).

(19C.2)

In general, the ordinary and extraordinary indices are increasing functions of ω and relation (19C.2) cannot be satisﬁed if both beams are either ordinary or extraordinary. However, Equation (19C.2) can be satisﬁed by using the ordinary wave at one frequency and the extraordinary wave at the other frequency. For a uniaxial negative crystal (such as KH2 PO4 , also called KDP), no (ω) must have a value between ne (2ω) and no (2ω). There are then directions of the wave-vector for which the ordinary index at angular frequency ω is equal to the extraordinary index at angular frequency 2ω. These directions form a cone of revolution around the optic axis (Exercise 17.6). They are said to produce phase matching. Second harmonic generation (SHG) is widely used, in particular to generate green light at wavelength 532 nm starting with a Nd:YAG laser which emits in the infra-red at 1064 nm.

Further reading G. New, Introduction to Non-Linear Optics (Cambridge University Press, 2011) A. Yariv, Y. Pochi, Optical Waves in Crystals (Wiley, 2003)

Chapter 20

Solutions to the exercises 20.1. Exercises for Chapter 2 Exercise 2.1 The ﬁgure below shows the plane perpendicular to the mirrors going through a given point M. O is the intersection of zz with this plane. M is the transform of M through m1 and M the transform of M through m2 . M”

O

Trace of M2 M’ M

Trace of M1

Figure 20.1 1.

We see that (OM, OM ) = 2α and m2 m1 = Rotzz (2α).

2.

By left-multiplying through m2 , we obtain m1 = m2 Rotzz (2α) since (m2 )2 = E with E being identity. In the same way, by right-multiplying by m1 and using (m1 )2 = E, we obtain m2 = Rotzz (2α)m1 .

3.

The existence of an n-fold axis zz leads to Rotzz (2π/n) being a symmetry operation. m1 is also assumed to be a symmetry operation. So is the product Rotzz (2π/n) m1 = m2 . Therefore there is a mirror M2 enclosing the angle π/n with M1 , etc.

4.

If A is the rotation by π/2 around the axis of the pyramid and m1 , m2 , m3 , m4 the operations of symmetry with respect to each of the 4 mirrors, the 8 symmetry operations are A, A2 , A3 , A4 = E, m1 , m2 , m3 , m4 .

5.

The symmetry group is not commutative. For example m1 m2 = A and m2 m1 = A3 if m1 and m2 are the mirror operations with respect to two mirrors deduced from each other through a 45◦ rotation around zz .

© Springer Science+Business Media Dordrecht 2014 C. Malgrange et al., Symmetry and Physical Properties of Crystals, DOI 10.1007/978-94-017-8993-6_20

435

436

Symmetry and Physical Properties of Crystals

Exercise 2.2 C2 H2 Br2 molecule: a 2-fold axis going through the line that connects the C atoms; 2 orthogonal mirrors going through the 2-fold axis, one containing the H atoms, the other the Br atoms. C3 H4 molecule: the ﬁgure below shows the projection, with the ordinates indicated, of the molecule onto a plane perpendicular to the carbon chain and going through the central C atom. It shows that there is a ¯4 axis going through the line that connects the carbons, with the center of symmetry of the rotoinversions coinciding with the central C atom. There are 2 orthogonal mirrors, with traces M1 and M2 , and two 2-fold axes in the plane of the ﬁgure and at 45◦ to the mirrors. M2 A2(0)

A2(0)

–u

C H

u

u

M1

–u

Figure 20.2

Exercise 2.3 The 4-fold axes are Ox, Oy and Oz, perpendicular to the faces and going through the center O of the cube (Fig. 20.3). The 3-fold axes are the major diagonals of the cube (DF, AG, CE and BH). The 2-fold axes connect the middles of two sides in two opposite faces. Consider, for example, the axis going through M, the middle of BC, and N the middle of EH. MN is parallel to EB. But EB is perpendicular to AF and to AD. Thus it is perpendicular to the plane ADGF. A rotation by π around MN thus transforms the cube apices A, D, G and F into G, F, A and D respectively. It is also clear that this rotation transforms C, B, E and H into B, C, H and E respectively. Thus the cube is transformed into itself. MN is a 2-fold axis.

20.2. Exercises for Chapter 3 Exercise 3.1 1.

The equation of the plane has form hx + ky + lz = n with n an integer. It goes through the nodes (1, 0, 0), (0, 1, 0) and (0, 0, 3), so that h = n, k = n, 3l = n. The required plane is (331).

2.

The (hkl) plane containing [211] and [120] satisﬁes equations 2h+k +l = 0 and h + 2k = 0, so that h = −2k and l = 3k. The plane is (¯213). It contains [302].

Chapter 20 – Solutions to the exercises

437

z D

C M

A

B O y

x

N

H

G

E

F

Figure 20.3 3.

The required row [uvw] satisﬁes equations 3u + v + w = 0 and u − v = 0. Thus u = v and 4u = −w. The row is [11¯4].

Exercise 3.2 1.

The required angle α is the angle between the normals, respectively n1 and n2 , to the planes (101) and (10¯1). n1 = [101]∗ and n2 = [10¯1]∗ . n1 · n2 = n1 n2 cos α with n1 = a∗ + c∗ and n2 = a∗ − c∗ . Since a∗ and c∗ are perpendicular: c2 − a2 a∗2 − c∗2 = = −0.413 and α = 114.4◦ . a∗2 + c∗2 c2 + a2 Another method can be used in this simple case where the planes (101) and (10¯1) are parallel to b and thus perpendicular to the plane of the ﬁgure, (c, a). We see immediately that tan γ = c/a so that γ = 32.8◦ . The angle 2γ = 65.6◦ is the supplement of α. cos α =

_ Trace of (101)

a

c

Trace of (101)

Figure 20.4 2.

In this system a∗ and b∗ are respectively parallel to a and b. Furthermore, a and b have the same norm, and the same applies to a∗ and b∗ . Therefore ha+kb is parallel to ha∗ +kb∗ , hence perpendicular to (hk 0). In contrast, a∗ and c∗ are respectively parallel to a and c but the ratios of their moduli are diﬀerent since a∗ = 1/a and c∗ = 1/c.

438 3.

Symmetry and Physical Properties of Crystals d321 =

1 . Thus d321 = 1.169 Å. 3a∗ + 2b∗ + c∗

Exercise 3.3 1.

(a) The equation of line D is hu + kv = n an integer, u and v being the coordinates of the nodes on D. 2h = n, 3k = n, so that n = 6 and h = 3, k = 2. The equation is 3u + 2v = 6. (b) 5 lines numbered from 1 to 5. (c) The rows have equation 3u + 2v = n. For the row going through node (1, 0), n = 3. For the row going through (0, 1), n = 2 (Fig. 20.5).

N

D

b M O

a

1

2

3

4

5

6

Figure 20.5 2.

(a) The row that goes through M and N is [2¯30]. Plane (hkl) is parallel to c, hence l = 0. It contains [2¯30], hence 2h − 3k = 0. The plane is (320). This result can be retrieved using the above ﬁgure. The lattice plane closest to origin intersects plane (a, b) along the line numbered 1, which intersects a at a/3 and b at b/2. (b) Plane of the form (32). MP parallel to [20¯1], hence = 6, so that the family is (326).

Exercise 3.4 1.

Figure 20.6a below, where c and c∗ are taken to point upwards. √ a∗ = b∗ = 2/a 3; c∗ = 1/c.

2.

Set V∗ = [110]∗ = a∗ + b∗ . (V∗ )2 = (a∗ + b∗ )(a∗ + b∗ ) = a∗2 + b∗2 + 2a∗ · b∗ = 3a∗2

Chapter 20 – Solutions to the exercises

439

Trace of (110) d110

b* b

b * O

a* a

O

(a)

a

(b)

Figure 20.6 since a∗ · b∗ = (a∗ )2 cos γ ∗ = (a∗ )2 /2.

d110

√

2 . a 1 a = = . [110]∗ 2

V∗ =

3a∗ =

This result can, in this special case, be retrieved geometrically using Figure 20.6b. 3.

Let α be the angle between the planes (120) and (100). It is also the angle between the vector [120]∗ , in other words a∗ + 2b∗ , and [100]∗ = a∗ . The calculation is: (a∗ + 2b∗ ) · a* = a∗ + 2b∗ a∗ cos α. √ This yields cos α = 2/ 7 and α = 40.9◦ .

Exercise 3.5 1.

a b

; Area OMN = × h k

a d

area OMQ = × ; h i

d b

area OQN = × . i k

b N

Q M O

a

d

Figure 20.7 2.

Area OMN = area OMQ + area OQN. Since the cross products have the same orientation, we can write: a b a d d b × = × + × h k h i i k

and d = −a − b.

440

Symmetry and Physical Properties of Crystals a×b a×b 1 a×b =− − and =− Therefore: hk hi ik hk hence h + k + i = 0.

3.

1 1 + hi ik

¯ (12¯31) plane; rotation 2π/3 (3121); rotation 4π/3 (2¯311); symmetry with respect to (a, c) (1¯321); symmetry with respect to (b, c) (¯3211).

Exercise 3.6 Unit cell EFGHKLMN. If there were nodes A, B, C and D at the centers of the faces EHNK, EFLK, FGML and HGMN respectively, then AB would be a lattice vector. But AB = NL/2, and there should be a node at the center of face KLMN, so that ﬁnally the lattice would be face-centered. N

M

K A

L D B H

E

C G

F

Figure 20.8 Exercise 3.7 CsCl has a cubic P lattice; the motif is: a pair of neighboring Cs+ and Cl− ions. NaCl has an F-centered cubic lattice; motif: one Na+ and a neighboring Cl− . ZnS has an F-centered cubic lattice; the motif is one Zn2+ and one neighboring S2− . Diamond has an F-centered cubic lattice with the motif: C at (0, 0, 0) and C at (1/4, 1/4, 1/4). CaF2 has an F-centered cubic lattice, with motif: Ca (0, 0, 0) and two F atoms, at (1/4, 1/4, 1/4) and −(1/4, 1/4, 1/4) respectively for example. TiO2 has a tetragonal P lattice, with a motif consisting of two TiO2 groups, one around the Ti at (0, 0, 0) and the other around the Ti at (1/2, 1/2, 1/2). CaTiO3 has a P cubic lattice; the motif is Ca at (0, 0, 0), Ti at (1/2, 1/2, 1/2) and 3 O at the centers of the three faces of the cubic unit cell, viz. at (0, 1/2, 1/2), (1/2, 0, 1/2), (1/2, 1/2, 0). It is clear that an atom in the motif can always be replaced by an identical atom displaced by a lattice vector. For example, in the motif indicated for CaF2 , the F atom at (−1/4, −1/4, −1/4) could be replaced by an F atom at (1/4, −1/4, 1/4) deduced through the lattice mode translation 1/2(a + c), etc. Exercise 3.8 1.

For clarity, the atoms of one layer at height 0 are represented by full circles, connected by full lines forming hexagons. Those of the following layer are represented by empty circles connected by dashed lines which also form hexagons. They are at height 1/2 (Fig. 20.9).

Chapter 20 – Solutions to the exercises

441

d b

height 0 height ½

a

Figure 20.9 2.

The cell is hexagonal, with a value of c equal to twice the distance between layers, viz. c = 6.70 Å. The distance atoms in √ two neighboring √ √ d between a layer is such that d = (2/3)a( 3/2) = a/ 3 and a = 3d = 2.46 Å. There are four atoms per unit cell.

Exercise 3.9 1.

Consider a prism. The two Gd atoms in the bases each is counted for 1/2. The 12 Ni atoms at the apices of the prism each count for 1/6, thus in total 2 atoms. The atoms at the centers of the 6 faces each count for 1/2, thus in total 3. The formula is GdNi5 .

2.

The lattice is hexagonal and the motif, comprising a GdNi5 group, is included in the shaded area on Figure 20.10. #

D

#

#

#

b

#

#

# #

#

C

#

a

B

b

# # #

A #

#

CD

O Gd at height 0 Ni at height 0 # Ni at height ½

a

# #

# #

AB

BC

Figure 20.10 3.

The face parallel to AB is a (110) plane, in hexagonal lattice notation (11¯20). The face parallel to BC is deduced from the face parallel to AB by a rotation through −2π/3 (or 4π/3), and the correct permutation of

442

Symmetry and Physical Properties of Crystals indices (k becomes h, h becomes i) leads to plane (1¯210). In the same way, the face parallel to CD, which is deduced from the face parallel to AB by a rotation through 2π/3, is a (¯2110) plane. These results can be checked on the reduced hexagonal lattice in Figure 20.10: the plane of the family closest to origin, intersecting vector a at a/h and vector b at b/k, has been represented for each face.

4.

The angle between the (1¯10) and (110) planes is equal to 90◦ .

Exercise 3.10 Projection of the nodes of a face-centered tetragonal lattice onto a plane perpendicular to c. 0

½

0

0

½

b ½

0

½

0 a1

b1 0

½

0

½ a

½

0

Figure 20.11 The unit cell deﬁned by the basis vectors a1 , b1 , c, half the size of the F(a,b) unit cell, is centered tetragonal. Note: the same projection applies for an F-centered cubic √ lattice, but then the centered lattice would have a c vector with length 2 times larger than a1 and b1 . It would no more be cubic. Exercise 3.11 Projection of the nodes of a face-centered monoclinic lattice onto a plane perpendicular to c, here chosen parallel to the 2-fold axis. 0

0

½

0

½

b2

½ 0

½

b

½

0

½

0

0

½

0

½

0

½

a1 0

½

b1

a2 0

0

½

½

a

Figure 20.12

0

Chapter 20 – Solutions to the exercises

443

The basis vectors a1 and b1 deﬁne a monoclinic centered unit cell and the vectors a2 and b2 = b1 a base-centered monoclinic unit cell (a2 , c), with B lattice. Exercise 3.12 Line zz , containing the major diagonal K F of the face-centered cubic unit cell, is a 3-fold axis (Fig. 20.13a). A rotation by 2π/3 around this axis changes L into G , G into K and K into L . The middle of L G , R , is transformed into the middle of G K, S , and in the same way S is changed into Q . Line zz therefore intersects the plane P containing the equilateral triangle L G K at its center of gravity I , which is also the center of gravity of the equilateral triangle R S Q . In the same way, zz intersects the plane P containing the equilateral triangle F GL at its center of gravity I. Figure 20.13b is a projection of the planes P and P along zz : the projections of the nodes in plane P are represented by full circles and those of plane P by empty circles. The respective positions of the projections of triangles F GL and L G K, whose centers of gravity I and I project at the same point, are easily deduced from the fact that lines F G and KL , GL and L G , and LF and KG are pairwise parallel. Figure 20.13b is identical to Figure 3.14c if it is complemented by the lattice translations. Since the lattice is face-centered cubic and not rhombohedral, √ the distance between the (111) planes is perfectly deﬁned and equal to a 3/3 if a is the length of the basis vectors. L’

K’

L

z’

R’ F’

L’

G’ I’

S

Q’

S

Q

c

z

S’

I

I

F

R # I’

R’

L b

K

Q'

K R

a

F’

G

S’ Q

G G’

(a)

(b)

Figure 20.13 Exercises 3.13 and 3.14 They should be addressed in the same way as used in the course to determine the reciprocal lattice of a face-centered cubic lattice. For the reciprocal lattice of a body-centered cubic lattice, we obtain a primitive cell with basis vectors A∗ = b∗ + c∗ ,

B∗ = c∗ + a∗ ,

C∗ = a∗ + b∗ ,

444

Symmetry and Physical Properties of Crystals

and thus a face-centered cubic lattice with basis vectors 2a∗ , 2b∗ and 2c∗ . The reciprocal lattice of an A (base-centered) lattice has a primitive cell with basis vectors A∗ = a∗ ,

B∗ = (b∗ − c∗ ),

C∗ = (b∗ + c∗ ).

The lattice is an A-type base-centered lattice, with basis vectors a∗ , 2b∗ and 2c∗ .

20.3. Exercises for Chapter 4 Exercise 4.1 Figure in plane Π : M H M1 V/2

P P’

H’ O V M2

Figure 20.14 O is the middle of M1 M2 = V. MM2 = MM1 + M1 M2 = 2(MH + M1 O) = 2(MH + V/2) = 2MH if HH = M1 O = V/2. Exercise 4.2 Consider a general point M. The ﬁgure is drawn in the plane going through M and perpendicular to zz . The traces of P1 and P2 are represented in this plane. 1.

An elementary geometrical argument shows that M2 is the transform of M through a symmetry with respect to O (Fig. 20.15a). P2 M

O M2

P2

A

M1

M

O

P1 M’1 V

P1 A

M1

M2

(a)

(b)

Figure 20.15 2.

M2 is the transform of M through the product operation (Fig. 20.15b). Line MM2 intersects the trace of P2 at A. Triangles MOA and MM1 M2

Chapter 20 – Solutions to the exercises

445

are similar. Since O is the middle of MM1 , we deduce that A is the middle of MM2 and that OA = M1 M2 /2 = V/2, independently of the choice of point M in the plane. M2 deduces from M through a rotation by π around an axis deduced from zz through a translation by V/2.

20.4. Exercises for Chapter 5 Exercise 5.1 1.

In plane Π, shown on Figure 20.16b, the projection H2 of M2 deduces from the projection H of M by a rotation through 2θ around zz . Also H2 M2 = −H1 M1 = HM, hence M2 deduces from M by a rotation through 2θ around zz . z H2

M2 x’

O

y’

H1

M H

M1

H1

y

x

y

x’

H2

y’

H

x

z’

(a)

(b)

Figure 20.16 2.

A A = R⊥ (2θ). By right-multiplying this equation with A and noting that A2 = E (where E is the identity operation), we ﬁnd: A = R⊥ (2θ)A. In the same way, left-multiplying by A and knowing that A 2 = E, we obtain A = A R⊥ (2θ). If an object has an n-fold axis zz , then Rzz (2π/n) is a symmetry operation for this object. If it additionally has a 2-fold axis perpendicular to zz , the operation of rotation by π around this axis xx , noted A, is also a symmetry operation. So is the product Rzz (2π/n)A. We just showed that Rzz (2π/n) A = A where A is a rotation by π around an axis perpendicular to zz and enclosing with axis xx an angle π/n. Repeating the argument, the object is shown to have n 2-fold axes, perpendicular to zz , and enclosing angles of π/n with each other.

Exercise 5.2 The stereographic projection of a general direction is shown on Figure 20.17a by the cross marked 1. Its transforms through rotations by 2π/3 and 4π/3 around the axis perpendicular to the projection plane are the crosses marked 2 and 3 respectively. The transforms of directions 1, 2 and 3 through the 2-fold axis whose stereographic projection consists of points A and B are the circles

446

Symmetry and Physical Properties of Crystals

marked 4, 5 and 6 respectively. This ﬁgure shows the existence of two 2-fold axes enclosing angles of 2π/3 and 4π/3 with AB (Fig. 20.17b). 6 2

1

A

B 4

5 3

(a)

(b)

Figure 20.17 Exercise 5.3 1.

We choose an orthonormal coordinate system (Oxyz) such that Oy and Oz coincide with the 4-fold axes (the origin O is therefore located at their intersection). We deﬁne the operators for rotation by an angle θ around, say an axis Oy as ROy (θ), which means that, if V is the vector obtained through rotation of a vector V by an angle θ around an axis Oy, then V = ROy (θ) V. The matrices representing the operators for rotations by ±π/2 around Oy or Oz, in the axis system we deﬁned, are given by: ⎛ ⎞ ⎛ ⎞ 0 −1 0 0 1 0 ROz (−π/2) = ⎝ −1 0 0 ⎠ ROz (π/2) = ⎝ 1 0 0 ⎠ 0 0 1 0 0 1 ⎛

⎞ 0 0 1 ROy (π/2) = ⎝ 0 1 0 ⎠ −1 0 0

⎛

⎞ 0 0 −1 ROy (−π/2) = ⎝ 0 1 0 ⎠ . 1 0 0 ⎛ ⎞ 0 0 1 We deduce that ROy (π/2)ROz (π/2) = ⎝ 1 0 0 ⎠. 0 1 0 The composition, or product operation, of a rotation by π/2 around Oz with a rotation by π/2 around Oy is an operation which transforms basis vector i into j, j into k and k into i, i.e. a rotation by 2π/3 around the axis parallel to direction [111] in a cube with sides parallel to Ox, Oy and Oz. The same result can be obtained by considering a cube ABCDEFGH (Fig. 20.18). The rotation by π/2 around Oz transforms: A, B, C, D, E, F, G, H into B, C, D, A, F, G, H, E respectively. The rotation by π/2 around Oy transforms: F, G, C, B, E, H, D, A into G, C, B, F, H, D, A, E respectively.

Chapter 20 – Solutions to the exercises

447

z D

C

A

B

O

y

H E

G F

Figure 20.18 We thus see that, through rotations around Oz, A becomes B and B, through rotation around Oy, becomes F. Thus the composition (product) of the two operations ﬁnally transforms: A, B, C, D, E, F, G, H into F, B, A, E, G, C, D, H respectively. Points B and H remain unaltered, and A becomes F, F becomes C and C becomes A. In the same way, E becomes G, G becomes D, D becomes E. The result is a rotation by 2π/3 around the axis [111] of the cube. In the same way, we can show using either method that: ROy ( π/2 ) ROz ( −π/2 ) = R[1¯11] (−2π/3), ROy ( −π/2 ) ROz ( π/2 ) = R[11¯1] (−2π/3), ROy (−π/2) ROz (−π/2) = R[¯111] (2π/3). Thus the directions [1¯11], [11¯1], [¯111] are also 3-fold axes. We show below the matrices representing rotations by 2π/3 around the four cube diagonals: R[111] (2π/3) ⎞ 0 0 1 ⎝ 1 0 0 ⎠ 0 1 0 ⎛

R[1¯11] (2π/3) ⎛

⎞ 0 −1 0 ⎝ 0 0 −1 ⎠ 1 0 0

R[11¯1] (2π/3) ⎛

⎞ 0 1 0 ⎝ 0 0 −1 ⎠ −1 0 0

R[¯111] (2π/3) ⎛

⎞ 0 −1 0 ⎝ 0 0 1 ⎠ −1 0 0

We recall that the operation inverse to the rotation by 2π/3 around one of these axes is the rotation by −2π/3 around the same axis, and that the associated matrix is the transpose of the matrix of the 2π/3 rotation. 2.

Performing the product of the operation consisting of a ±2π/3 rotation around one of the major diagonals of the cube by the operation consisting

448

Symmetry and Physical Properties of Crystals of a ±2π/3 rotation around another cube diagonal, we obtain a rotation by π around Ox or Oy or Oz. Example: ⎛ ⎞⎛ ⎞ 0 −1 0 0 0 1 R[1¯11] (2π/3)R[111] (2π/3) = ⎝ 0 0 −1 ⎠ ⎝ 1 0 0 ⎠ 1 0 0 0 1 0 ⎛ ⎞ −1 0 0 = ⎝ 0 −1 0 ⎠ 0 0 1 i.e. a rotation by π around Oz.

Exercise 5.4 Let K be the point in the stereographic projection which is located at the intersection of arc bFb and line aa . This point K is the stereographic projection of the direction parallel to row [011] and pointing to the north, i.e. direction OP on Figure 20.19b. This ﬁgure shows the meridian plane containing√direction [011]. We obtain: OK = R tan(π/8) = √ = R tan α = R tan(θ/2) √ R( 2 − 1). Therefore aK = R 2. Since ab = R 2, the circle that goes through b , K and b has for its center a. b’ c’

P

F a

K

a’

a

F’

O

c

K = 45°

b

(a)

(b)

Figure 20.19 Exercise 5.5 Crystals with a hexagonal lattice can have either a hexagonal or a rhombohedral point group. The groups are as follows: Holohedral: 6/mmm, order 24; Hemihedral: ¯62m, 6mm, 622, 6/m and ¯3m with order 12; Tetartohedral: ¯6, 6, 3m, 32, ¯3 with order 6; Ogdohedral: 3, with order 3. The reader can check that the only cases of ogdohedral crystals are those with point group 3 and with a hexagonal lattice. Exercise 5.6 1.

Form {31¯40} (a) Group 6mm: to ﬁnd the faces equivalent to face (hkil) through the symmetry operations of group 6mm, it is suﬃcient to apply the various

Chapter 20 – Solutions to the exercises

449

symmetry elements of the group, viz. rotations by kπ/3 (k being an integer between 1 and 6), and then a mirror operation on the various faces obtained, hence 6 new faces. This gives a total of 12 planes if the normal to the planes is not a special direction. The indices are obtained by remembering that plane hkil intersects axes Ox, Oy and Ov, parallel respectively to a, b and d, at a/h, b/k and d/i. Rotations by 2π/3 and 4π/3 thus produce permutations among h, k and i and conserve l. Rotations by an odd number of ¯ k¯¯il) and the planes deduced through times π/3 lead to the form (h ¯ k¯ and ¯i. permutations among h, (hkil) becomes (ihkl) through a rotation by 2π/3. It becomes (kihl) ¯ through a rotation by through a rotation by 4π/3. It becomes (k¯¯ihl) ¯ kl) ¯ through a rotation ¯ ¯ ¯ π/3, (hk il) through a rotation by π and (¯ih by 5π/3. The operation of a mirror parallel to c and a conserves h and l and exchanges k and i. ¯ (4310), ¯ ¯ ¯ 30), ¯ Form {31¯40} comprises 12 planes: planes (3140), (1430), (14 (3¯¯140), (4¯3¯10) and their transforms through one of the mirrors, (3¯410), (¯4130), (13¯40), (¯1¯340), (¯34¯10), (4¯1¯30). (b) Group ¯62m: the planes equivalent to (31¯40) are obtained by applying ﬁrst the symmetry operations associated to the ¯6 axis, i.e. rotations by 2π/3 and 4π/3 around Oz, and a mirror perpendicular to Oz. The mirror symmetry transforms (hkil) into (hki¯l). Here l = 0 and plane (31¯40) is a special plane because its normal is in the mirror plane. We must also consider the second generating element, which can be either one of the 2-fold axes or one of the mirrors. We choose a mirror, which we take to be parallel to a. Form {31¯40} comprises 6 planes: the planes (31¯40), (¯4310), (1¯430) and (3¯410), (¯4130), (13¯40). 2.

Form {111} for the cubic groups. Form {111} contains the set of faces perpendicular to all the directions equivalent to direction [111]∗ . For a general direction, the number of equivalent directions is equal to the order n of the group. If the direction is located on a symmetry element to which are associated p symmetry operations, the number of equivalent directions is equal to n/p. Direction [111]∗ is a three-fold axis in all the cubic groups. Furthermore, in those groups which also contain diagonal mirrors, i.e. groups ¯43m and m¯3m, it is also located on these mirrors, which divides by another factor 2 the number of equivalent directions. Note that, in this enumeration, it is suﬃcient to consider one of the 3 diagonal mirrors, because the two other mirrors are only the result of the existence of the 3-fold axis and of a mirror going through this axis.

450

Symmetry and Physical Properties of Crystals Group 23: form {111} comprises plane (111) and planes (1¯1¯1), (¯11¯1) and (¯1¯11), obtained by applying the 2-fold axes. It is distinct from form {¯1¯1¯1} because there is no center of symmetry. The latter form contains planes (¯1¯1¯1), (¯111), (1¯11) and (11¯1). We ﬁnd 4 equivalent planes. This number is indeed equal to n/p = 12/3 = 4. Group m¯3: the existence of the mirrors entails the existence of a center of symmetry. The forms {111} and {¯1¯1¯1} are identical and comprise the eight planes (111), (1¯1¯1), (¯11¯1), (¯1¯11) and (¯1¯1¯1), (¯111), (1¯11), (11¯1). We check that this number is equal to n/p = 24/3 = 8. Group 432: although this group does not feature a center of symmetry, the forms {111} and {¯1¯1¯1} are identical because, for this special direction, the product of a rotation by π around Ox and a rotation by π/2 around Oy transforms direction [111]∗ into direction [¯1¯1¯1]∗ . The eight planes are equivalent (n/p = 24/3 = 8). Group ¯43m: same results as for 23. Forms {111} and {¯1¯1¯1} are diﬀerent. The order of the group is 24. Direction [111]∗ is a 3-fold axis and is located on a diagonal mirror, hence 24/6 = 4 equivalent directions. ¯ Group m3m: eight equivalent planes (48/6), and the forms {111} and {¯1¯1¯1} are equivalent because there is a center of symmetry.

20.5. Exercises for Chapter 7 Exercise 7.1 1.

(a) Generating elements: ¯4 and 2-fold axes. The stereographic projection is performed onto a plane perpendicular to the ¯4-axis (Fig. 20.20a). Consider a general direction, with stereographic projection at 1 (cross), and its transforms 2 (circle), 3 (cross), and 4 (circle) through the symmetry operations associated to the ¯4-axis. The 2-fold axis has for its stereographic projection points A and B. The transforms of directions 1, 2, 3 and 4 through rotations by π around the 2-fold axis have stereographic projections 5, 6, 7 and 8 respectively. This shows the existence of the other 2-fold axis and of two mirrors at 45◦ to the 2-fold axes. ¯ Generating elements: 4-axis, and the mirror with the segment MM as its stereographic projection. Same approach: 1, 2, 3 and 4 are the stereographic projections of directions equivalent through the operations associated with the ¯4 axis. 5, 6, 7 and 8 are respectively the stereographic projections of the transforms of directions 1, 2, 3 and 4 through the mirror operation m. This shows the existence of the 2-fold axes located in the projection plane at 45◦ to the projections of the mirrors. The stereographic projection shows very clearly that, if an object has a ¯4 axis and a mirror containing this axis, then there are also 2-fold axes in a plane perpendicular to the ¯4 axis, going through

Chapter 20 – Solutions to the exercises

451

the center of symmetry associated to this ¯4 axis, and enclosing an angle of 45◦ with the traces of the mirrors in this plane (see the C3 H4 molecule of Exercise 2.2). (b) The stereographic projections of the equivalent directions of group 4/mmm, the point group of the tetragonal lattice, are given on Figure 20.20c, where the initial general direction is identical to that in Figures 20.20a and 20.20b. We see that Figures 20.20a and 20.20b represent subgroups of 20.20c. The basis vectors a and b of the lattice are parallel to the mirrors of group 4/mmm, and can therefore be parallel either to the 2-fold axes or to the mirrors of group ¯42m, leading to the space groups P¯42m and P¯4m2 respectively. 2 8 A

7 3

77

2 8 1 5

B

M

7 3

1 5

6 4

6 4

(a)

(b)

P– P42m

7 7

M’

7 7 77

(c)

P– P4m2

Figure 20.20 In order to determine all the symmetry elements present in the unit cell, we apply the rules for the product (composition) of symmetry operations (rotations and rotoinversion) with the lattice translations (Sect. 7.2.3), keeping in mind that a ¯4 axis contains a 2-fold axis. The positions equivalent to the general position with coordinates x, y, z are: ¯ P42m x, y, z y, x ¯, z¯ x ¯, y¯, z y¯, x, z¯ x, y¯, z¯ y, x, z x ¯, y, z¯ y¯, x ¯, z . ¯ P4m2 x, y, z y, x ¯, z¯ x ¯, y¯, z y¯, x, z¯ ¯, z¯ x, y¯, z y, x, z¯. x ¯, y, z y¯, x For both groups, the four positions in the ﬁrst line are obtained by applying the ¯4 operations and their multiples. Those of the second line are obtained by applying to the ﬁrst four positions the operation

452

Symmetry and Physical Properties of Crystals rotation by π around an axis parallel to a for P¯42m, and the operation mirror parallel to a for P¯4m2.

2.

Same approach as in (1). The point group 6/mmm of the hexagonal lattice contains 6 mirrors going through the 6-fold axis, which gives rise to two possibilities for placing the mirrors of point group 3m, a subgroup of the point group of the lattice. If the lattice is rhombohedral, the point group ¯3m of the lattice only has 3 mirrors going through the 3-fold axis. They must coincide with the mirrors in the point group of the crystal.

Exercise 7.2 Group P4 contains a 4-fold axis. We choose the origin of the unit cell on this 4-fold axis, and apply the rules of Section 7.2.3 to obtain the product of the symmetry operations associated to the 4-fold axis with the lattice translations. The rotation by π/2 around the 4-fold axis at A, followed by a translation a, is equivalent to a rotation by π/2 around an axis going through K. There is a 4-fold axis at K. The operation rotation by π around the 4-fold axis going through A followed by a translation a is equivalent to a rotation by π around an axis going through L, the middle of AB = a. There is a 2-fold axis at L, etc. C

K

b

K

b L M

A

L

B

A A

B a I4

a P4

Figure 20.21 Group I4. Existence of a 4-fold axis and a translation 1/2(a + b + c). To perform the product of a rotation by π/2 around the 4-fold axis going through A with the translation, we decompose the translation into its component parallel to the axis, viz. c/2, and its component perpendicular to the axis, 1/2(a + b) = AK. The result is a rotation by π/2 around an axis located at L, the middle of AC = b (the point on the perpendicular bisector of AK at which AK subtends an angle π/2) followed by a translation by c/2. Therefore there exists a 42 axis going through L the middle of AC. The product (composition) of the rotation by π around the 4-fold axis going through A with the translation 1/2(a + b + c) is a rotation by π followed by a translation by c/2 around an axis going through M the middle of AK, hence there exists a 21 axis going through M.

Chapter 20 – Solutions to the exercises

453

Exercise 7.3 The generating elements of this space group are the operations (m1 , c/2) and (m2 , a/2) (modulo the lattice translations). The common origin O of these two operations is located at a point on the intersection of these two mirrors. The product of these two symmetry operations with the same origin is performed by applying relation (4.8). We obtain: (m1 , c/2)(m2 , a/2) = (m1 m2 , m1 a/2 + c/2) = (A, −a/2 + c/2), where A is a rotation by π around the intersection line of the two mirrors. The translation part includes both a component (c/2) parallel to the axis, which is a 21 axis, and a component perpendicular to the axis, (−a/2). The latter can be canceled by displacing the axis: for a 2-fold axis, this implies translating it by −a/4 (ﬁgure below). Thus there is a 21 axis at O such that OO = −a/4. The space group is written Pca21 (c-type mirror perpendicular to a, a-type mirror perpendicular to b, and 21 axis parallel to c). O’ b

O

M1

O’

a

M2

Figure 20.22 Exercise 7.4: Np 1.

Primitive lattice, since the atomic positions cannot be separated into various groups deduced from one another through one (or several) lattice mode translations, such as 1/2(a + b) for a C lattice, etc.

2.

The Np atom at A is located on a 4¯ axis, and we easily see two perpendicular pure mirrors going through A (Fig. 20.23a). The point group of this site is therefore ¯42m. The Np atom at B is on a 4-fold axis and on two orthogonal pure mirrors. The site of atom B has point group 4mm. The point group of the crystal has subgroups ¯ 42m and 4mm. It is therefore 4/mmm.

3.

There is therefore a mirror parallel to the plane of the ﬁgure. It is a glide mirror with translation 1/2(a + b) at height 0 (n-type mirror). The diagonal mirrors going through A are glide mirrors with glide 1/2(a + b) but those which go through B are pure mirrors. The space group is therefore P4/nmm (n◦ 129 in International Tables vol. A). Figure 20.23b shows the

454

Symmetry and Physical Properties of Crystals mirrors present in the unit cell, and the rotation and rotoinversion axes perpendicular to the plane of the ﬁgure. 0

u

u

–u

0

0

u

0

u

–u

0

–u

0

0

–u

A

B

0

B

A

(a)

(b)

Figure 20.23 Exercise 7.5: NiAs Primitive lattice (same reason as in Exercise 7.4, question (1)). A 63 axis going through a Ni atom, 3 pure mirrors going through this 63 axis, and 3 c-type mirrors (glide c/2) intersecting them. Space group P63 mc (n◦ 186 in I.T. A) (the mirrors perpendicular to a and b are m-type mirrors).

1.

½,0

½,0

½,0

u

½,0

u+½

½,0

½,0

u

u

S

u

u+½ ½,0

½,0

b Ni As

½,0

u

½,0

u u+½

½,0

D

R

u+½

a

(a)

b

u+½ ½,0

½,0

u+½ ½,0

b

½,0

u

u u+½

½,0

a

(b)

u+½ ½,0

A

F

K

P

B a

C Q

½,0

(c)

Figure 20.24 Figure (c) shows the symmetry axes and the mirrors present in the unit cell. We apply the rules of Section 7.2.3, taking into account the fact that a 63 axis contains a 3-fold axis and a 21 axis. The combination of the 3-fold axis at P and of the lattice translation a gives a 3-fold axis at point K, while the combination of axis 21 at P and of the lattice translation a gives a 21 axis at B. In order to ﬁnd the eﬀect of the combination of the pure mirror with trace SQ and of the lattice translation a, we decompose a into its component parallel to the mirror, (a − b)/2, and its component perpendicular to the mirror, (a + b)/2. The result is the operation of a

Chapter 20 – Solutions to the exercises

455

mirror with glide (a − b)/2, the trace of which on the plane of the ﬁgure deduces from SQ through a translation by (a + b)/4. We obtain the glide mirror with trace CD (dotted line, see Tab. 7.2). The combination of the c-mirror with trace PR and of the translation with vector a is equivalent to a mirror with trace BC (translation by half the component perpendicular to the mirror of vector a) with glide equal to the component parallel to the mirror of a, viz. (a + b)/2, which adds to c/2 to yield a mirror with trace BC and glide (a +b + c)/2 (dotted line with long/short alternation). The point symmetry of the Ni site is 6mm and that of the As atoms is 3m. Exercise 7.6: FeOCl 1.

Primitive lattice (same reason as in Exercise 7.4, question (1)).

2.

b

w

–u

w

–u

w

u

–w

u

–w

u

w

–u

w

–u

w

Fe

Cl

a w=v

O

w = v’

Figure 20.25 3.

We immediately distinguish two pure mirrors perpendicular to the plane of the ﬁgure and perpendicular to each other. There is a glide mirror with glide vector 1/2 (a + b), parallel to the plane of the ﬁgure at height 0, and therefore a n mirror perpendicular to c. The space group is Pmmn. The associated point group is mmm, a centrosymmetric group. There are therefore symmetry centers. The 2-fold axes parallel to c are pure axes while those parallel to a or b are 21 axes.

4.

There are 8 positions (order of the group = 8) equivalent to the general position. Their coordinates are: x, y, z

x + 1/2, y + 1/2, −z

−x, y, z

−x + 1/2, y + 1/2, −z

x, −y, z

x + 1/2, −y + 1/2, −z

−x, −y, z

−x + 1/2, −y + 1/2, −z.

456

Symmetry and Physical Properties of Crystals

20.6. Exercises for Chapter 8 Exercise 8.1 Figure 3.14b, reproduced below, shows a rhombohedral unit cell. In the closepacked structure ABCABC, points L, N, P and M are the centers of identical, mutually contacting atoms with radius ρ. Then LN = LP = PN = 2ρ. The angle of the rhombohedron is then equal to 60◦ . A rhombohedron with angle 60◦ is the primitive cell for a face-centered cubic lattice. T 3 R S

2

1

Q

N

M

P

0

L

Figure 20.26 Exercise 8.2 1.

Figure 20.27a shows the regular tetrahedron MNPL formed by the centers M, N and P of three mutually contacting atoms in a plane A and the center L of the atom in plane B which contacts them. H, the projection of L onto plane A, is the center of gravity (and orthocenter)√of the equilateral triangle MNP, and MH = (2/3)MK. Also MK = a( 3/2), hence √ MH = a/ 3. L L

h M

O

P a

H

(a)

K N

M

H

(b)

Figure 20.27 In the right triangle LHM, h2 = ML2 – MH2 = a2 (2/3). Hence h = a 2/3.

Chapter 20 – Solutions to the exercises 2.

457

2 = 1.63. c = 2h = 2a 2/3 and c/a = 2 3

Exercise 8.3 1.

2.

3.

We use the ﬁgures and the results of Exercise 8.2. The center O of the tetrahedron with side a is located on the altitude LH, which is a 3-fold axis for the tetrahedron. We must have OL = OM = d (Fig. 20.27b). OH = h − d = a 2/3 − d, OM2 = d2 = MH2 + OH2 = a2 /3 + (a 2/3 − d)2 = d2 . a 3 2 . We deduce from the last equation: a − 2a 2/3d = 0 and d = 2 2 Comparing d and h, we see that d = 3h/4. The center of the regular tetrahedron is located on the height from a vertex, at a distance from the vertex equal to 3/4 of the height. " # a 3 3 d= = r1 + r2 and r2 = a/2 hence r1 = a/2 −1 2 2 2 r1 3 − 1 = 0.225. and = r2 2 The positions of the Zn atoms are those of the centers of an ABABAB stacking. The calculated value of c/a is 1.636. The stacking of the centers is that of close packing, but here the atoms are not in contact. The value of parameter u is close to 0.375 = 3/8. 0

0

0

½ 0

½ 0

0

½ 0

½ 0

0

Figure 20.28 The heights indicated on the ﬁgure are those of the Zn atoms represented by full circles. The S atoms (empty circles) project onto the Zn atoms and are located a distance 3c/8 above them. A Zn atom at height 0 and the 3 neighboring Zn atoms at height 1/2 form a regular tetrahedron with height c/2. The S atom at height 3/8 is a distance 3c/8 from the vertex, hence 3/4 of the height of the tetrahedron. It is therefore at the center of this tetrahedron. The wurtzite structure can thus be represented as an ABABAB stacking, with S atoms in the tetrahedral sites. There is one tetrahedral site per Zn atom. In the blende structure, the Zn atoms form

458

Symmetry and Physical Properties of Crystals an f.c.c. stacking, i.e. an ABCABC stacking. The S atoms are in every other tetrahedral site, since there are twice as many tetrahedral sites as Zn atoms in the f.c.c. structure. We thus understand more clearly why ZnS can exist under these two forms, blende and wurtzite.

20.7. Exercises for Chapter 9 Exercise 9.1 ⎛ 1. 2.

−1 ⎜ √23 {aij }= ⎝ − 2 0

√ 3 2 − 12

0

⎞ 0 ⎟ 0 ⎠ 1

√ T11 = (1/4) T11 + (3/4) T22 − ( 3/2) T12 = T11 √ hence (3/4) (T22 − T11 ) = ( 3/2) T12 , √ = (3/4) T11 + (1/4) T22 + ( 3/2) T12 = T22 T22 √ hence (3/4) (T22 − T11 ) = ( 3/2) T12 , √ = ( 3/4) (T11 − T22 ) − (1/2) T12 = T12 T12 √ hence ( 3/4) (T22 − T11 ) = (−3/2) T12 .

(20.1) (20.2) (20.3)

Relations (20.1) and (20.2) are identical. Relations (20.2) and (20.3) imply that T12 = 0 and T11 = T22 . 3.

√ √ = (−1/2) T13 + ( 3/2)T23 = T13 hence 3 T13 = 3 T23 , T13 √ √ T23 = (− 3/2) T13 − (1/2) T23 = T23 hence 3 T23 = − 3 T13 , = T33 . T33

We deduce that T13 = T23 = 0. Exercise 9.2 Since [T ] is a material tensor, each component must remain unchanged under a symmetry operation of the point group of the crystal, i.e. Tij = Tij . The operation of a mirror perpendicular to Ox1 changes the xi coordinates of a point M into coordinates xj such that: x1 = −x1

x2 = x2

x3 = x3 .

Since the components Tij transform like the product of coordinates xi xj , we obtain: =T , =T , =T , T22 T33 T11 11 22 33 =T . T12 = −T12 = T12 = 0, T13 = −T13 = T13 = 0, T23 23

Chapter 20 – Solutions to the exercises

459

We see that the components Tij with the subscripts ij containing one and only one subscript equal to 1 are zero. The operation of a mirror perpendicular to Ox2 changes the coordinates xi of a point M into coordinates xj such that: x1 = x1

x2 = −x2

x3 = x3 ,

and the components Tij containing one and only one subscript equal to 2 are zero. The existence of a third mirror entails that the components containing one and only one subscript equal to 3 are zero. But these components, T13 and T23 , are already zero because of the ﬁrst two mirrors. We thus note that the form of the tensor is the same for groups mm2 and mmm: ⎞ ⎛ T11 ⎠ ⎝ T22 T33 in an orthonormal set of axes perpendicular to the mirrors.

20.8. Exercises for Chapter 10 Exercise 10.1 ⎛ 1.

2.

⎞ 0 −4 2 0⎠ 0 3 ⎞ 0 4 2 0 ⎠ 0 3

1 {Tij } = ⎝ 0 −4 ⎛ 1 {Tij } = ⎝ 0 4

We could expect to ﬁnd the tensor unchanged, since the basis vector b, perpendicular to a and c, is a 2-fold axis for the three monoclinic groups. Exercise 10.2 ⎛ 1.

⎞ 7 (a) j = ⎝ √0 ⎠ E 3 ⎛ 7+√3 ⎞

⎜ (d) j = ⎝

√

2

0

√ 5+ √ 3 2

⎟ ⎠E

⎛

⎞ 0 (b) j = ⎝ 8 ⎠ E 0 ⎛ √ ⎞ 3

⎛ √ ⎞ 3 (c) j = ⎝ 0 ⎠ E 5 ⎛ √ ⎞ 3

⎜ 2 ⎟ ⎜ 2 ⎟ (e) E = ⎝ 0 ⎠ E ; j = ⎝ 0 ⎠ 8E = 8E, 1 2

1 2

j is parallel to E, and this special direction for E is that of one of the principal axes of the tensor.

460 2.

Symmetry and Physical Properties of Crystals (a) jn = 5E. (b) jn /E = 5 is the value of the electrical conductivity of the material in direction [001].

3.

The coordinate change matrix is given by: √ ⎞ ⎛ 3 1 0 − ⎟ ⎜ 2 2 ⎟ ⎜ ⎜ 0 1 0 ⎟ ⎟. ⎜√ ⎠ ⎝ 3 1 0 2 2 The form of the tensor is therefore: ⎛ 4 8 σ =⎝

⎞ ⎠ 8

and this axis system is that of the principal axes of the tensor. This result is no surprise, since the initial form of the tensor shows that Ox2 is a principal axis. Furthermore, we saw in question 1e) that the direction in plane (Ox3 , Ox1 ) that encloses an angle of 60◦ with Ox3 is a principal axis. Exercise 10.3 ⎛ 1.

{σij } = ⎝

⎞

σ1 ⎛

2.

⎠ (see Sect. 10.5.4).

σ1

σs = (s1 s2 s3 ) ⎝

σ3

⎞⎛

σ1 σ1

⎞ ⎞ ⎛ s1 σ1 s 1 ⎠ ⎝ s2 ⎠=(s1 s2 s3 ) ⎝ σ1 s2 ⎠ σ3 s3 σ3 s 3

= σ1 (s21 + s22 ) + σ3 s23 . s1 = sin θ cos ϕ,

s2 = sin θ sin ϕ,

s3 = cos θ.

σs = σ1 sin2 θ + σ3 cos2 θ. σs is independent of ϕ. This is no surprise since the representative quadric for tensor [σ] has revolution symmetry around the three-fold axis. Exercise 10.4 1.

The symmetry operation associated to the presence of a 4¯ axis parallel to Ox3 is the product of a rotation by π/2 around this axis by a symmetry with respect to origin O. This operation changes the coordinates xi of a point M into coordinates xj such that: x1 = −x2

x2 = x1

x3 = −x3 .

Chapter 20 – Solutions to the exercises

461

The components Tij are expressed as: T11 = T22

T22 = T11

T33 = T33 ,

T13 = T23

T23 = −T13 .

T12 = −T21 = −T12 (symmetric tensor),

Because [T ] is a material tensor, each component must remain unchanged under an operation of the point group of the crystal: Tij = Tij . We deduce: T11 = T22

⎛

The form of tensor [T ] is: ⎝

T12 = 0 T11

T13 = T23 = 0. ⎞ ⎠.

T11 T33

2.

¯ For group 42m, we must add another mirror perpendicular to axis Ox1 . The symmetry operation with respect to the mirror changes the coordinates xi of a point M into coordinates xj such that: x1 = −x1 ,

x2 = x2 ,

x3 = x3 .

This operation leaves the form of the tensor unchanged.

20.9. Exercises for Chapter 11 Exercise 11.1 1.

In a coordinate system (Ox1 x2 x3 ) has the form: ⎛ T ⎝ 0 0

where Ox1 is parallel to n, tensor [T ] ⎞ 0 0 0 0 ⎠. 0 0

In the coordinate system (Ox1 x2 x3 ), the components Tij of the stress = a a T since the only non-zero tensor are given by Tij = aik ajl Tkl i1 j1 = T . The only components which play a role are the term Tij is T11 components ai1 of the matrix for going over from system (Ox1 x2 x3 ) to system (Ox1 x2 x3 ), i.e. the components n1 , n2 , n3 of vector n. We obtain Tij = ni nj T , i.e. the matrix: ⎛ ⎞ n21 n1 n2 n1 n3 ⎝ n1 n2 n22 n2 n3 ⎠ T. n1 n3 n2 n3 n23 Exercise 11.2 1.

Tn = [T ]n. Here only T33 = 0 and (Tn )3 = n3 T and (Tn )2 = (Tn )1 = 0. Tν = Tn · n = n23 T.

462

Symmetry and Physical Properties of Crystals The shear component is the projection of Tn onto the surface. In the plane deﬁned by Tn and n (shown in the ﬁgure): τ 2 = Tn 2 − Tν2 = n23 T 2 − n43 T 2 = n23 T 2 (1 − n23 ), τ = T n3 1 − n23 .

T

Tn n

Figure 20.29 2.

√ 1 − 2n23 ∂τ = T , which vanishes for n3 = ± 2/2. 2 ∂n3 1 − n3 n3 = cos θ where θ is the angle between n and Ox3 . The shear stress is maximal for the orientations of the surface for which the normal is on a cone with axis Ox3 and apical angle 45◦ . Its value is then τ = T /2.

Exercise 11.3 The coordinate change matrix for the axis system is given by: ⎞ ⎛ √ √ 2 2 0 2 2 ⎟ ⎜ √2 √2 ⎝ − 2 0 ⎠. 2 0 0 1 In the new referential, the components Tij form the matrix: ⎛

T ⎝ 0 0

0 −T 0

⎞ 0 0 ⎠. 0

Exercise 11.4 1.

Direction Ox3 is a principal axis, with principal value 7.6. In the subspace (Ox1 , Ox2 ), we solve: det ({Tij } − λE) = 0. We obtain: λ1 = −2, λ2 = 5.5. For λ1 = −2, the principal direction is deﬁned by the relation x1 = −1.33 x2 between its components, so that the direction encloses an angle −36.9◦ with axis Ox1 .

Chapter 20 – Solutions to the exercises

463

For λ2 = 5.5, the principal direction is perpendicular to the above direction. Thus, the principal directions deduce from directions Ox1 and Ox2 through a rotation by −36.9◦ around axis Ox3 . 2.

The position of the center C of the Mohr circle is given by: xC = (2.8 + 0.7)/2 = 1.75 and angle 2θ is deﬁned by: tan 2θ = 3.6/(2.8 − 1.75), so that 2θ = 73.74◦ . Thus the principal directions deduce from directions Ox1 and Ox2 by a rotation through θ = −θ = −36.9◦ around axis Ox3 . P 3.6

2 ’

C –2

O

2.8

5.5

Figure 20.30 3.

√ Let n be the vector ( 3/2, 1/2, 0). We have (Tn )i = Tij nj , so that: ⎞ ⎛ ⎞ ⎛ √3 ⎞ ⎛ ⎞ ⎛ 0.7 3.6 0 2.4 (Tn )1 2 ⎝ (Tn )2 ⎠ = 107 ⎝ 3.6 2.8 0 ⎠ ⎝ 1 ⎠ = 107 ⎝ 4.5 ⎠ 2 0 0 7.6 0 (Tn )3 0 and Tn = 5.1 × 107 N m−2 . The value of the normal stress is: Tν = T · n =

and Tν = 4.3 × 107 N m−2 . The shear stress has value: τ =

√

3 2

1 2

0

⎛

⎞ 2.4 ⎝ 4.5 ⎠ 107 0

Tn 2 − Tν2 = 2.7 × 107 N m−2 .

20.10. Exercises for Chapter 12 Exercise 12.1 ⎛ 1.

⎛ ⎞ ⎞ 2 −1 0 2 12 0 {eij } = ⎝ 2 −2 0 ⎠ 10−5 ; {Sij } = ⎝ 12 −2 0 ⎠ 10−5 ; 0 0 0 0 0 0

464

Symmetry and Physical Properties of Crystals ⎛

0 − 32 {Ωij } = ⎝ 32 0 0 0

⎞ 0 0 ⎠ 10−5 . 0

[Ω] represents a rotation around n (0, 0, 1) through an angle

2.

(see Sect. 12.2.2). ⎛ ⎞ 1 Δ 1 n = √13 ⎝ 1 ⎠ and = ni nj Sij = 10−5 . n 3 1

3 −5 10 rad 2

Exercise 12.2 1.

The displacement vectors Δu = Δr − Δr associated to each side have the following values: ⎛ ⎞ 0 For the side parallel to Ox1 : Δux1 = ⎝ S ⎠. 0 ⎛ ⎞ S For the side parallel to Ox2 : Δux2 = ⎝ 0 ⎠. 0 A square with unit side becomes a lozenge, the major diagonal of which is parallel to the diagonal of the undeformed square (ﬁgure below). x2

S

S O

x1

Figure 20.31 2.

We want to ﬁnd the eigenvalues and eigenvectors of the matrix {Sij } associated to the tensor: ⎛ ⎞ 0 S 0 {Sij } = ⎝ S 0 0 ⎠ . 0 0 0 The eigenvalues are found by solving det ({Sij }−λE) = 0. We obtain three distinct principal values: λ1 = S, λ2 = −S and λ3 = 0. The eigenvector associated to λ1 is parallel to the vector (1, 1, 0), the eigenvector associated

Chapter 20 – Solutions to the exercises

465

to λ2 is parallel to vector (−1, 1, 0). The eigenvector associated to λ3 is along Ox3 . The frame of the principal axes is rotated by 45◦ around Ox3 with respect to the initial frame. In this axis system, the matrix representing the tensor is: ⎛ ⎞ S 0 0 ⎝ 0 −S 0 ⎠ . 0 0 0 Exercise 12.3 ⎛ ⎞ cos α ΔL ⎝ ⎠ = ni nj Sij = η cos2 α − 0.3η sin2 α 1. n = sin α , L n 0 ΔL so that = η(1.3 cos2 α − 0.3). For α < 61.3◦ , L > L. L n ⎛ ⎞ cos α 2. After deformation, Δu = [S]Δr and Δr = ⎝ sin α ⎠ L, so that 0 Δu1 = ηL cos α

and

Δu2 = −0.3ηL sin α.

We project this displacement ⎛ vector Δu ⎞ onto the direction perpendicular − sin α to the direction deﬁned by ⎝ cos α ⎠ (Fig. 20.32). 0 x2 u L

x1

O

Figure 20.32 We obtain: −ηL cos α sin α − 0.3ηL cos α sin α = −1.3η cos α sin αL and the expression for angle ε is: ε = −1.3η cos α sin α = −0.65η sin 2α. Exercise 12.4 ⎛ 4 −1 Sij = ⎝−1 1 2 0

⎞ 2 0⎠ 10−6 , 3

⎛

⎞ 0 3 −4 Ωij = ⎝−3 0 0 ⎠ 10−6 . 4 0 0

466

Symmetry and Physical Properties of Crystals

From the results of Section 12.2.2, the rotation axis is parallel to the unit vector n, with direction cosines n1 , n2 , n3 such that n1 Δα = 0, n2 Δα = −4 × 10−6 and n3 Δα = −3 × 10−6 , where Δα is the rotation angle. The rotation is performed around the direction of unit vector ⎛ ⎞ 0 ⎜ 4⎟ n = ⎝− 5 ⎠ . − 35

We can rewrite matrix {Ωij } in the form: ⎛

0

⎜ 3 ⎝− 5 4 5

3 5

− 45

⎞

0

⎟ 0 ⎠ 5 × 10−6

0

0

and Δα has the value Δα = 5 × 10−6 rad around n. Exercise 12.5 1.

The form of the thermal expansion tensor is ⎞ ⎛ α1 ⎠ ⎝ α1 α3 in an orthonormal set of axes (Ox1 x2 x3 ) where Ox3 is parallel to the basis vector c of the hexagonal structure and Ox1 is any direction in the plane (a, b).

1 a100 − a20 = −1.5 × 10−6 ◦ C−1 , α1 = α2 = a20 ΔT

1 c100 − c20 = 28 × 10−6 ◦ C−1 . α3 = c20 ΔT

2.

Let s be a unit vector with arbitrary direction. Its components in spherical coordinates are: s1 = sin θ cos ϕ,

s2 = sin θ sin ϕ,

s3 = cos θ.

The value of the thermal expansion in direction s is given by: ⎛ ⎞⎛ ⎞ α1 s1 ⎠ ⎝ s2 ⎠ = α1 sin2 θ + α3 cos2 θ. αs = (s1 , s2 , s3 ) ⎝ α1 α3 s3 α3 α3 2 + pπ (p an integer). or θ0 = ± arctan αs = 0 if tan θ0 = − α1 |α1 |

Chapter 20 – Solutions to the exercises

467

By deﬁnition, 0 < θ0 < π and θ0 = 77◦ or θ0 = 103◦ , i.e. all directions on a cone with apex O and apical angle 77◦ . The representative surface for this tensor comprises a one-sheet hyperboloid and a two-sheet hyperboloid. These two hyperboloids are tangent to the same cone with angle 2θ0 and with the apex at the origin of the axes. In the directions of the cone which is the asymptote to the hyperboloids, the relative elongation is zero because the radius vector r tends toward inﬁnity. 3.

We consider the direction ϕ = 0, θ = θ0 i.e. the unit vector s (sin θ0 , 0, cos θ0 ). The displacement vector Δu has components (α1 sin θ0 , 0, α3 cos θ0 ). It is easy to check that Δu · s = α1 sin2 θ0 + α3 cos2 θ0 = 0. The rotation angle ε we want to determine is equal to the norm of Δu. 1/2

cos2 θ0 Δu = (α21 sin2 θ0 + α23 cos2 θ0 )1/2 = |α1 sin θ0 | 1 + tan4 θ0 2 sin θ0 = |α1 sin θ0 | (1 + tan2 θ0 )1/2 = |α1 | |tan θ0 | Thus Δu = 1.3 arcsec ◦ C−1 .

α3 |α1 | and ε is equal to 6.48 × 10−6 rad ◦ C−1

Exercise 12.6 Δa Δc = α11 ΔT and = α33 ΔT . a c Let ϕ be the angle between the planes (100) and (101) (ﬁgure below). ( 10 1) a

O

(100)

c

Figure 20.33 We have: tan ϕ =

a , or ϕ = 57.21◦ . c

Hence: d(tan ϕ) Δϕ 2Δϕ Δa Δc = = = − = (α11 − α33 )ΔT. tan ϕ sin ϕ cos ϕ sin 2ϕ a c We get: α11 − α33 = −2.1 × 10−6 ◦ C−1 . On the other hand, the volume expansion is 23.4 × 10−6 so that: 2α11 + α33 = 23.4 × 10−6 ◦ C−1 .

468

Symmetry and Physical Properties of Crystals

Solving this system of equations, we obtain: α11 = 7.1 × 10−6 ◦ C−1 and α33 = 9.2 × 10−6 ◦ C−1 . Exercise 12.7 1.

Tetragonal phase between 0 and 120◦ C: 1 Δa = 2.3 × 10−5 , ΔT a 1 Δc = = −2.7 × 10−5 . ΔT c

Δa = 0.011 Å and α11 = α22 = Δc = −0.013 Å and α33

The thermal expansion tensor is: ⎛ ⎞ 2.3 ⎝ ⎠ 10−5 ◦ C−1 . 2.3 −2.7 Let n be any direction with direction cosines n1 , n2 and n3 . The value αn of α in direction n is given by: αn = ni αij nj , so that: αn = α11 (n21 + n22 ) + α33 n23 which vanishes for −

α33 n2 + n2 = 1 2 2. α11 n3

If n is expressed in spherical coordinates (θ, ϕ), then tan2 θ = −α33 /α11 = 1.171 and the angle between the direction we want to determine and Ox3 is (±47.3◦ + p 180◦ ), hence 47.3◦ or 132.7◦ . 2.

From Figure 20.34, we have: α bo = bm cos 2 2

co

α co = bm sin . 2 2

bo

cm

bm

Figure 20.34 For the orthorhombic unit cell at T = 0◦ C, α = 90.20◦ and we obtain: ao = 3.988 Å,

bo = 5.664 Å,

co = 5.684 Å.

For the orthorhombic unit cell at T = −100◦ C, α = 90.40◦ and we obtain: ao = 3.978 Å,

bo = 5.654 Å,

co = 5.694 Å.

Chapter 20 – Solutions to the exercises

469

The thermal expansion tensor in the orthorhombic phase can be written, in the orthonormal axis system parallel to the basis vectors of the orthorhombic unit cell: ⎛ ⎞ 2.5 ⎝ ⎠ 10−5 ◦ C−1 . 1.8 −1.8 3.

(a) Cubic ↔ tetragonal transition at 120◦ C: In an orthonormal axis system parallel to the basis vectors of the cubic unit cell, the strain tensor is: ⎛ ⎞ −2 ⎝ ⎠ 10−3 . −2 2.7 (b) Strain tensor describing the transition from the cubic unit cell at 120◦ C to the orthorhombic unit cell at 0◦ C: The orthorhombic unit cell must be compared with the equivalent unit cell in the cubic phase, i.e. with a double unit cell with basis vectors a , b and c . a is parallel to a and a = 4.010 Å, b and c are parallel respectively to the diagonals of the (b, c) faces, and such that √ b = c = a 2 = 5.671 Å. The strain tensor is diagonal in an axis system parallel to the basis vectors of the orthorhombic unit cell, and: ao − a = −5.5 × 10−3 , a co − c = = 2.2 × 10−3 . c

S11 = S33

S22 =

bo − b = −1.2 × 10−3 , b

The strain tensor, when expressed in the axis system of the orthorhombic unit cell, is thus ⎛ ⎞ −5.5 ⎝ ⎠ 10−3 . −1.2 2.2 (c) Strain tensor describing the transition from the cubic unit cell to the rhombohedral unit cell: When going over from the cubic unit cell to the rhombohedral unit cell, the [111] axis of the cube remains a 3-fold axis, and the mirrors containing this axis (the diagonal mirrors of the cube) remain mirrors for the rhombohedral unit cell. The basis vectors a = OA and c = OC of the cubic unit cell become vectors OA and OC such that: ⎧ ⎧ √ ϕ2 2 ⎪ ⎪ ⎨ a (1 −√ 2 ) ⎨ a ϕ √2 and OC OA a ϕ √22 a ϕ 22 ⎪ ⎪ 2 ⎩ ⎩ 2 aϕ 2 a (1 − ϕ2 )

470

Symmetry and Physical Properties of Crystals where ϕ is the angle of rotation of a, b and c in their respective diagonal mirror (Fig. 20.35).

C

c

C’

B’ B

b a

O

A’ A

Figure 20.35

S11 = S22 = S33 = √ 2 . S12 = S13 = ϕ 2

a − a a (1 − ϕ2 /2) − a ≈ = −3.5 × 10−3 . a a

Calculating angle of α, we obtain OA · OC = √ ϕ as a function cos α 2 2 √ a cos α = a ϕ 2 and ϕ = 2 . cos α = 1.2 × 10−3 . 2 The component S23 is obtained in the same way.

Thus S12 = S13 =

The strain tensor describing the transition from the cubic unit cell to the orthorhombic unit cell, expressed in the axis system parallel to the basis vectors of the cubic unit cell, is: ⎛ ⎞ −3.5 1.2 1.2 ⎝ 1.2 −3.5 1.2 ⎠ 10−3 . 1.2 1.2 −3.5

20.11. Exercises for Chapter 13 Exercise 13.1 By adding to the symmetry elements of group ¯42m a 3-fold axis parallel to the major diagonal of a cube with sides parallel to the basis vectors a, b and c, we obtain point group ¯43m. Such a symmetry operation changes the coordinates xi of a point M into coordinates xj such that: x1 = x2 We obtain: s11 = s22 = s33 ,

x2 = x3

x3 = x1 .

s44 = s55 = s66 ,

s12 = s13 = s23 .

Chapter 20 – Solutions to the exercises

471

Exercise 13.2 1.

We choose an orthonormal axis system (Ox1 x2 x3 ) parallel to the basis vectors a, b and c of the cubic unit cell. From the generalized Hooke’s law, Sα = sαβ Tβ with T1 = T and T2 = T3 = T4 = T5 = T6 = 0. The resulting strain tensor is: ⎞ ⎛ s11 ⎠ T. ⎝ s12 s12 The relative elongation in direction [100] is s11 T .

2.

In the axis system (Ox1 x2 x3 ), rotated through 45◦ around Ox3 with re = T and that spect to the initial frame, the stress tensor is such that T11 the other components are zero. In the frame (Ox1 x2 x3 ) linked to ⎛ T /2 ⎝ T /2 0

the cube axes, this tensor becomes: ⎞ T /2 0 T /2 0 ⎠ 0 0

and the strain tensor is thus:1 ⎛ s44 s11 + s12 2 ⎜ s44 Sij = ⎜ + s12 s 11 ⎝ 2

⎞ ⎟T ⎟ . ⎠2 2s12

The relative elongation in direction [110] is obtained through relation (12.12): Δ = wi wj Sij . w T Δ = [2(s11 + s12 ) + s44 ]. We obtain: [110] 4 3.

If the solid is isotropic, these two strains must be identical, so that: 1 [2(s11 + s12 ) + s44 ] = s11 4

or

s44 = 2(s11 − s12 ).

Exercise 13.3 We directly apply the generalized Hooke’s law (relation (13.1a)): Sα = sαβ Tβ with T1 = T2 = T3 = −p and T4 = T5 = T6 = 0, using the elasticity tensor for group 4/mmm given in Table 13.5. We obtain : ⎞ ⎛ s11 + s12 + s13 ⎠. s11 + s12 + s13 −p ⎝ 2s13 + s33 1. We recall that S12 = S21 = S6 /2.

472

Symmetry and Physical Properties of Crystals

The numerical values are: S11 = S22 = −0.61 × 10−4 ; S33 = −0.68 × 10−4 ΔV and = S11 + S22 + S33 = −1.9 × 10−4 . V Exercise 13.4 We consider a uniaxial stress T , parallel to a direction w with direction cosines w1 , w2 and w3 . In an orthonormal axis system (Ox1 x2 x3 ) where Ox1 is = T. parallel to w, the stress tensor has a single non-zero component, T11 Let Tij be the components of this tensor in the axis system (Ox1 x2 x3 ) parallel to the cube axes. We have Tmn = aim ajn Tij where {aij } is the transformation matrix for going over from system (Ox1 x2 x3 ) to system (Ox1 x2 x3 ). =a Here Tmn = a1m a1n T11 1m a1n T with a11 = w1 , a12 = w2 and a13 = w3 .

T11 = w12 T,

T22 = w22 T,

T33 = w32 T,

T12 = w1 w2 T, T13 = w1 w3 T, T23 = w2 w3 T. We showed (Sect. 12.4) that:

ΔV = S11 + S22 + S33 . V

S11 = s11 T11 + s12 (T22 + T33 ) = s11 w12 T + s12 T (w22 + w32 ),

S22 = s11 T22 + s12 (T11 + T33 ) = s11 w22 T + s12 T (w12 + w32 ), S33 = s11 T33 + s12 (T11 + T22 ) = s11 w32 T + s12 T (w12 + w22 )

ΔV = [s11 (w12 + w22 + w32 ) + 2s12 (w12 + w22 + w32 )]T = (s11 + 2s12 ) T V since w12 + w22 + w32 = 1.

and

Exercise 13.5 It was shown in Section 13.7 that, in the cubic system, the reciprocal of Young’s modulus in a given direction, deﬁned by unit vector w with components w1 , w2 and w3 , is given by: 1 s44 2 2 (w2 w3 + w12 w22 + w12 w32 ) = A. = s11 − 2 s11 − s12 − Ew 2 Ew has its maximum value if A is minimum. If s11 − s12 − s44 /2 is positive, A is minimum if B = w22 w32 + w12 w22 + w12 w32 is maximum. In spherical coordinates (θ, ϕ), the components of w are: w1 = sin θ cos ϕ, 2

w2 = sin θ sin ϕ, 4

w3 = cos θ

sin θ sin 2 θ + sin2 2 ϕ . 4 4 B is the sum of two terms which are always positive, and only the second term depends on ϕ. Therefore B is maximum, whatever the value of θ is, when sin2 2ϕ is maximum, hence for 2ϕ = π2 + pπ i.e. ϕ = π4 + p π2 .

and

B=

Chapter 20 – Solutions to the exercises For this value of ϕ,

B=

473

sin2 2 θ sin4 θ + . 4 4

dB = cos 2θ sin 2θ + cos θ sin3 θ dθ = 2 cos3 θ sin θ − sin3 θ cos θ = sin θ cos θ(3 cos2 θ − 1).

√ = 0 for θ = 0, θ = π/2 and for θ such that cos θ = 1/ 3, thus θ = 54.7◦ , which is the angle between direction [111] and Ox3 in the cubic system. dB dθ

For θ = 0 : π For θ = : 2 Pour θ = 54,7◦ :

B=0 B = 1/4 B = 1/3, the maximum value.

This shows that the value of Young’s modulus for a cubic material is extremal in direction [111]. Exercise 13.6 In an orthonormal coordinate system (Ox1 x2 x3 ) where direction Ox1 is parallel to the [110] direction of the cubic lattice, the stress tensor has only one non-zero = T. component, T11 In the orthonormal frame (Ox1 x2 x3 ) with the cubic unit cell, this tensor becomes: ⎛ T /2 T /2 ⎝ T /2 T /2 0 0

axes parallel to the basis vectors of ⎞ 0 0 ⎠. 0

The resulting strain is given, in the axis system of the cube, by: ⎛ ⎞ s44 s11 + s12 2 ⎜ ⎟T s44 ⎟ . Sij = ⎜ s11 + s12 ⎝ ⎠2 2 2s12 We recall that S6 = 2S12 = 2S21 . The relative elongation in a given direction is given by (12.12): Δ = wi wj Sij . w Δ = w12 S11 + w22 S22 + 2w1 w2 S12 + w32 S33 . We obtain: Here, w Δ Δ T s44 s11 + s12 + , = = s12 T, [110] 2 2 [001] T s44 Δ s . = + s − 11 12 [1¯10] 2 2

474

Symmetry and Physical Properties of Crystals

Numerically: s12 = −6× 10−13 m2 N−1 , s11 = 9.6× 10−12 m2 N−1 , s44 = 78× 10−12 m2 N−1 . Exercise 13.7 1.

The uniaxial stress applied to the crystal is parallel to direction [111], with √ unit vector w, with direction cosines w1 = w2 = w3 = 1/ 3. In a coordinate system where Ox1 is parallel to [111], the only non-zero = T . In the orthonormal coordinate component of the stress tensor is T11 system with axes parallel to the basis vectors of the cubic unit cell, this tensor becomes (see the solution to Exercise 11.1): ⎞ ⎛ T T T 1⎝ T T T ⎠. 3 T T T

2.

The resulting strains are: S1 = S2 = S3 =

3.

T (s11 + 2s12 ), 3

S4 = S5 = S6 =

T s44 . 3

The basis vectors a, b, c of the cubic unit cell become respectively, after deformation, the vectors a , b , c such that ⎛ ⎛ ⎛ ⎞ ⎞ ⎞ 1 + S1 S6 /2 S6 /2 a = ⎝ S6 /2 ⎠ a, b = ⎝ 1 + S1 ⎠ a, c = ⎝ S6 /2 ⎠ a. S6 /2 S6 /2 1 + S1 We note that the components of these vectors can be deduced from one another by circular permutation. Therefore these vectors deduce from one another by rotation through 2π/3 around direction [111]. The unit cell has become rhombohedral. The parameter a of the rhombohedral unit cell is given by: T a = a(1 + S1 ) = a 1 + (s11 + 2s12 ) . 3 a · b = a b cos γ . Neglecting the second order terms, we obtain: cos γ = S6 = cos(π/2 − ε) = sin ε,

so that

ε = S6 =

T s44 . 3

Exercise 13.8 1.

In an orthonormal coordinate system (Ox1 x2 x3 ) with axes parallel to the sides of the parallelepiped, the uniaxial stress has only one non-zero component, T11 = −T . The resulting strain tensor is: ⎞ ⎛ s11 ⎠ T. s12 −⎝ s12

Chapter 20 – Solutions to the exercises

475

ΔL = −s11 T = −1.49 × 10−2 and ΔL = −74.5 μm L Δ = −s12 T = 0.63 × 10−2 and Δ = 6.3 μm. The orthonormal axis system (Ox1 x2 x3 ), with axes parallel to the sides of the rectangle parallelepiped, is deduced from the crystallographic axis system (Ox1 x2 x3 ) by a rotation through +45◦ around Ox3 . In the axis system (Ox1 x2 x3 ), the tensor has only one non-zero component, T11 = −T . In the coordinate system (Ox1 x2 x3 ), this tensor becomes ⎛ ⎞ −T /2 −T /2 ⎝ −T /2 −T /2 ⎠. 0 As a result,

2.

The components of the corresponding strain tensor are:

T = S2 , S3 = −s12 T, S1 = (s11 + s12 ) − 2 T and S6 = − s44 . S4 = S5 = 0 2 In the coordinate system (Ox1 x2 x3 ), these components become: T S1 = − [2(s11 + s12 ) + s44 ] = −0.76 × 10−2 , 4 T S2 = − [2(s11 + s12 ) − s44 ] = 0.63 × 10−2 , 4 S3 = −s12 T = 0.975 × 10−3 . S4 = S5 = S6 = 0. Since the non-diagonal terms are zero, the rectangle parallelepiped remains a rectangle parallelepiped. The sides AB and BC have changed respectively by Δ(AB)= −7.6 μm and Δ(BC) = 6.3 μm. Length L has changed by ΔL = 0.49 μm.

20.12. Exercises for Chapter 14 In all exercises, use is made of Table 14.1 to determine the Christoﬀel matrix, and of Tables 13.5a and 13.5b to know which components of the stiﬀness tensor [c] are non-zero. Exercise 14.1 1.

(a) k is parallel to [001]. In the orthonormal coordinate system (Ox1 x2 x3 ) where Ox3 is parallel to c, s1 = s2 = 0 and s3 = 1, so that Christoﬀel’s matrix is given by ⎞ ⎛ c55 c45 c35 ⎝ c45 c44 c34 ⎠ . c35 c34 c33

476

Symmetry and Physical Properties of Crystals From Table 13.5a, c35 = c34 = 0 ⎛ c55 ⎝ c45 0

and the matrix becomes: ⎞ c45 0 c44 0 ⎠ . 0 c33

(b) The propagation velocities are obtained from the eigenvalues of this matrix. They are given by: λ1 λ2 and v2 = v1 = ρ ρ with λ1,2 =

c44 + c55 ±

(c44 − c55 )2 + 4c245 , 2 c33 . v3 = ρ

The wave which propagates at velocity v3 is polarized parallel to direction [001]: it is a longitudinal wave. The waves which propagate with velocities v1 and v2 are transverse waves. The polarization of the wave with velocity v1 encloses with direction Ox1 , in plane (Ox1 ,Ox2 ), an angle θ1 such that:

(c44 − c55 ) − (c44 − c55 )2 + 4c245 λ1 − c55 θ1 = arctan = arctan . c45 2c45 The polarization of the wave with velocity v2 encloses with direction Ox1 the angle θ2 such that:

λ2 − c55 . θ2 = arctan c45 We check that θ2 − θ1 = π/2. 2.

For the orthorhombic system, c45 = 0 (see Tab. 13.5a). Christoﬀel’s matrix takes the form: ⎞ ⎛ c55 0 0 ⎝ 0 c44 0 ⎠ . 0 0 c33 Waves with polarization parallel to Ox1 and Ox2 , hence transverse, propagate with the respective velocities v1 and v2 , given by: c55 c44 v1 = and v2 = . ρ ρ

Chapter 20 – Solutions to the exercises

477

The wave with polarization parallel to Ox3 , hence longitudinal, propagates with velocity v3 given by: c33 v3 = . ρ 3.

Christoﬀel’s matrix is : ⎞ c55 c45 c35 ⎝ c45 c44 c34 ⎠ . c35 c34 c33 ⎛

From Tables 13.5a and 13.5b, all point groups with an axis of order larger than 2 feature c45 = c35 = c34 = 0. Furthermore, c44 = c55 . Christoﬀel’s matrix thus becomes: ⎛ ⎞ c44 ⎝ ⎠. c44 c33 There is a longitudinal wave, with propagation velocity v given by: c33 v = . ρ The transverse waves have their polarization along any direction in the plane (Ox1 , Ox2 ) and they propagate with velocity vt given by: c44 vt = . ρ 4.

For a general propagation direction in plane (Ox1 , Ox2 ), we have: s1 = 0, s2 = 0 and s3 = 0. Christoﬀel’s matrix is: ⎞ ⎛ Γ11 Γ12 ⎠ ⎝ Γ12 Γ22 Γ33 since Γ13 = Γ23 = 0 for a hexagonal crystal. Here: Γ11 = c11 s21 + c66 s22 ,

Γ22 = c66 s21 + c22 s22 ,

Γ33 = c55 s21 + c44 s22 = c44 (s21 + s22 ) = c44 , Γ12 = (c12 + c66 )s1 s2 . One wave with polarization parallel to the 6-fold axis can propagate. It is transverse, with propagation velocity given by: c44 . v= ρ

478

Symmetry and Physical Properties of Crystals

Exercise 14.2 1.

k is parallel to [100], hence s1 = 1, s2 = s3 = 0, and Christoﬀel’s matrix contains only 3 coeﬃcients: Γ11 = c11 , Γ22 = c44 , Γ33 = c44 . One longitudinal wave can propagate, with velocity v given by: c11 v = . ρ The transverse waves have any polarization direction in the plane (Ox2 , Ox3 ), and their propagation velocity vt is given by: c44 . vt = ρ

2.

√ k is parallel to [111], hence s1 = s2 = s3 = 1/ 3, and Christoﬀel’s matrix takes the form: ⎞ ⎛ c + 2c44 c12 + c44 c12 + c44 1 ⎝ 11 c12 + c44 c11 + 2c44 c12 + c44 ⎠ . 3 c12 + c44 c12 + c44 c11 + 2c44 The propagation velocities are obtained from det({Γij } − λE) = 0. If we set (c11 + 2c44 )/3 = a and (c12 + c44 )/3 = b: det({Γij } − λE) = (a − λ)[(a − λ)2 − b2 ] − b2 [a − λ − b] + b2 [b − (a − λ)]. We must solve: (a − λ)(a − λ + b)(a − λ − b) − 2b2 (a − λ − b) = 0, (a − λ − b)[(a − λ)(a − λ + b) − 2b2 ] = 0. We ﬁnd λ1 = a − b and λ2 − λ(2a + b) + a2 + ab − 2b2 = 0, so that λ2 = a − b = λ1 and λ3 = a + 2b. The eigenvector associated to λ3 = a + 2b turns out to be parallel to [111], so that the wave is longitudinal with propagation velocity: c11 + 2c12 + 4c44 v = . 3ρ The other two eigenvalues are equal and correspond to transverse waves with any polarization direction in the plane perpendicular to [111]. Their propagation velocity is given by: c11 − c12 + c44 . vt = 3ρ

Chapter 20 – Solutions to the exercises 3.

479

Numerically: The velocity of the transverse waves found in question (1) yields c44 : c44 = 4.40 × 1011 N m−2 . c11 and c12 are determined from the results of (2): c11 + 2c12 = 3ρv2 − 4c44 c11 − c12 = 3ρvt2 − c44 . We ﬁnd: c11 = 10.9 × 1011 N m−2 and c12 = −3.18 × 1011 N m−2 .

Exercise 14.3 1 The wave-vector k is parallel to [110]: s1 = s2 = √ and s3 = 0. 2 ⎞ ⎛ 0 c + c66 c12 + c66 1 ⎝ 11 Christoﬀel’s matrix is: 0 ⎠. c12 + c66 c11 + c66 2 0 0 2c44

c11 − c12 c11 + c12 + 2c66 −λ −λ . det({Γij } − λE) = (c44 − λ) 2 2 The propagation velocities are obtained from det({Γij } − λE) = 0. Here c44 is an eigenvalue with eigenvector [001]. c44 , polarization [001], transverse wave; We ﬁnd: v1 = ρ c11 − c12 v2 = , polarization [¯110], transverse wave; 2ρ c11 + c12 + 2c66 v3 = , polarization [110], longitudinal wave. 2ρ

20.13. Exercises for Chapter 15 Note: in this section, the coeﬃcients of the piezoelectric tensors which vanish are represented by small dots. Exercise 15.1 The piezoelectric tensor for group 422 has the following form in an orthonormal axes system (Ox1 x2 x3 ) where Ox3 is parallel to the 4-fold axis and Ox1 and Ox2 are parallel to the 2-fold axes: ⎛ ⎞ . . . . . d14 ⎝. . . . − d14 . ⎠ . . . . . . 0 To determine the form of the tensor for group 432, we just have to add a 3-fold axis, parallel to the diagonal of the cube, because the 2-fold axes perpendicular

480

Symmetry and Physical Properties of Crystals

to the diagonal planes result from the existence of the 4-fold and 3-fold axes. We then use the direct inspection method applied to a rotation by 2π/3 around the major diagonal of the cube. This operation changes the coordinates xi of a point M into coordinates xj such that: x1 = x2 ,

x2 = x3 ,

x3 = x1 .

We obtain: d14 = 2d132 = 2d213 = d25 = −d14 = d14 ,

whence d14 = 0.

Exercise 15.2 1.

(a) We consider the stereographic projection of the equivalent directions for group 222 (Fig. 20.36a). The Ox1 axis is parallel to one of the 2-fold axes. If we add the operation of symmetry with respect to a mirror enclosing an angle of 45◦ with Ox1 , we add the equivalent directions 5, 6, 7 and 8, which are the transforms of directions 1, 2, 3 and 4 respectively. We see that this leads to group ¯42m. 6 5 3 4

1 2

x1

3 4

1 2 8 7

(a)

(b)

(c)

Figure 20.36 The form of the piezoelectric tensor for group 222 (in an orthonormal set of axes parallel to the 2-fold axes) is (Tab. 15.2): ⎞ ⎛ . . . . d14 . ⎝. . . . d25 . ⎠ . . . . . . d36 The operation of symmetry with respect to the mirror changes the coordinates xi of a point M into coordinates xj such that: x1 = x2 ,

x2 = x1 ,

x3 = x3 .

This leads to d132 = d231 = d132 whence d25 = d14 . The transformation of d312 tensor is: ⎛ . . ⎝. . . .

yields nothing more. The form of the ⎞ . . d14 . . . d14 . ⎠ . . . . d36

Chapter 20 – Solutions to the exercises

481

(b) In the same way, considering subgroup mm2, the addition of the rotation by π around an axis at 45◦ to the mirrors leads to group ¯42m. The form of the tensor for group mm2 (in an orthonormal system with axes perpendicular to the mirrors) is: ⎞ ⎛ . . . . d15 . ⎝ . . . d24 . .⎠ . . . d31 d32 d33 . A rotation by π around an axis at 45◦ to the mirrors changes coordinates xi of a point M into coordinates xj such that: x1 = x2 ,

x2 = x1 ,

x3 = −x3 .

Therefore: d131 = −d232 = d131 whence d15 = −d24 ;

d311 = −d322 = d311 whence d31 = −d32 ; d333 = −d333 = d333 whence d33 = 0. The form of the tensor is: ⎛ ⎞ . . . . d15 . ⎝ . . . −d15 . .⎠ . . . . d31 −d31 . 2.

The tensor which we obtained in (1a), relative to an axis system (Ox1 x2 x3 ), must now be expressed in a new axis system (Ox1 x2 x3 ), deduced from the ﬁrst one through a rotation by 45◦ around axis Ox3 . Knowing the form of the tensor in the new axes reduces the task to the calculation of two of them: d15 and d31 . We apply the rule dijk = ail ajm akn dlmn , √ ⎛ √ 2 2 ⎜ 2 2 ⎜ √ √ ⎜ 2 ⎜− 2 ⎝ 2 2 0 0

where matrix {aij } has the form: ⎞ 0⎟ ⎟ ⎟. 0⎟ ⎠ 1

We obtain: d15 = 2d131 = (d132 + d231 ) =

d14 + d25 = d14 2

so that d15 = d14 = 0.17 × 10−11 C N−1 . d31 = d311 = whence d31 =

d36 d312 + d321 = 2 2

d36 = 2.6 × 10−11 C N−1 . 2

482

Symmetry and Physical Properties of Crystals

Exercise 15.3 For group 422 (as well as for group 622), the form of the piezoelectric tensor, in the orthonormal axis system (Ox1 x2 x3 ) where Ox3 is parallel to the 4-fold axis (or the 6-fold axis) and Ox1 and Ox2 are parallel to the 2-fold axes, has the form: ⎞ ⎛ . . . . . d14 ⎝. . . . −d14 . ⎠ . . . . . . 0 We saw (Sect. 15.3.4) that the longitudinal piezoelectric surface is deﬁned by the set of points P such that the length of the vector OP, parallel to the direction of the unit vector s (s1 , s2 , s3 ), is given by si sj sk dijk (Eq. (15.25)). Here, the only coeﬃcients playing a part are d14 = d123 + d132 and d25 = d213 + d231 = −d14 . We ﬁnd: OP = s1 s2 s3 (d14 + d25 ) and, since d25 = −d14 , we have OP = 0. The longitudinal piezoelectric surface vanishes for all directions. Exercise 15.4 The form of the piezoelectric tensor, for group 32, in the orthonormal axis system (Ox1 x2 x3 ) deﬁned in the text, is: ⎞ ⎛ . . d11 −d11 . d14 ⎝ . . . . −d14 −2d11 ⎠ . . . . . . . 1. (a) In the orthonormal system (Ox1 x2 x3 ), rotated by angle θ with respect to (Ox1 x2 x3 ), the applied stress tensor has only one non-zero = T. component, T11 In the frame (Ox1 x2 x3 ), this tensor becomes: ⎛ ⎞ cos θ sin θ 0 cos2 θ ⎝ cos θ sin θ sin2 θ 0 ⎠ T. 0 0 0 We ﬁnd for the components of polarization P: ⎞ ⎛ ⎞ ⎛ d11 (cos2 θ − sin2 θ) d11 cos 2θ ⎠ T = ⎝ −d11 sin 2θ ⎠ T. −d11 sin 2θ P=⎝ 0 0 Its norm is: P = d11 T of θ.

cos2 2θ + sin2 2θ = d11 T . It is independent

(b) P encloses with direction Ox1 the angle ϕ such that ϕ = −2θ. Thus the polarization rotates twice as fast as the stress in the plane(Ox1 , Ox2 ), and in the opposite direction.

Chapter 20 – Solutions to the exercises

483

(c) From question (1a), we see that P will be parallel to Ox2 if cos 2θ = 0, hence when θ = π/4 + p π/2 with p an integer. It is therefore suﬃcient to apply a uniaxial stress at 45◦ to the axes Ox1 and Ox2 . 2.

We saw that d111 = si sj sk dijk (Eq. (15.25)), so that here: d111 = s1 d111 (s21 − 3s22 ). Neither d14 nor d25 = −d14 are involved, since the corresponding terms vanish. In spherical coordinates (θ, ϕ), we obtain: d111 = d111 sin3 θ(cos3 ϕ − 3 sin2 ϕ cos ϕ) = d111 sin3 θ cos 3ϕ. The intersection of this surface with the plane (Ox1 , Ox2 ) is obtained for θ = π/2 and d111 = d111 cos 3ϕ (Fig. 20.37, showing d111 /d111 ). The curve is periodic vs ϕ, with period 2π/3, in agreement with the presence of the 3-fold axis. x2 1

–1

0

1

x1

–1

Figure 20.37

Exercise 15.5 1.

The piezoelectric tensor for ⎛ . ⎝. .

group ¯43m is given by: ⎞ . . d14 . . . ⎠. . . . d14 . . . . d14

Due to the form of this tensor, we must apply T4 = T23 , or T5 = T13 , or T6 = T12 . 2.

Using (15.25):

d111 = si sj sk dijk = 3s1 s2 s3 d14

so that d111 = 3d14 cos θ sin2 θ cos ϕ sin ϕ =

3 d14 cos θ sin2 θ sin 2ϕ. 2

484 3.

Symmetry and Physical Properties of Crystals d111 is maximal for ϕ = π/4 + p π/2 (p an integer) and for

∂d111 = 0. ∂θ

3 3 ∂d111 = d14 sin 2ϕ sin θ(2 cos2 θ − sin2 θ) = d14 sin 2ϕ sin θ(3 cos2 θ − 1) ∂θ 2 2 which vanishes for sin θ = 0 so that θ = 0 or π but, for these values, d111 is zero, hence minimal. √ d111 is maximal for 3 cos2 θ −1 = 0, hence cos θ = 1/ 3, or θ = 54.7◦ . This value of θ, along with ϕ = 45◦ , are the spherical coordinates of direction [111] in the cube. 4.

In the orthonormal set of axes (Ox1 x2 x3 ) parallel to the basis vectors of the cubic unit cell, the only non-zero component of strain is S6 , with S6 = d14 E. The strain tensor can be written as: ⎞ ⎛ d14 E 0⎟ ⎜ 0 2 ⎟ ⎜d E . ⎜ 14 0 0⎟ ⎠ ⎝ 2 0 0 0 The relative volume variation is given by the trace of this tensor, hence ΔV = 0. V To determine the new shape of the solid, we express the tensor in a coordinate system where Ox1 is parallel to [110], Ox2 is parallel to [¯110] and Ox3 is unchanged. The transformation matrix from the referential (Ox1 x2 x3 ) to this frame is: √ ⎞ ⎛√ 2 2 0⎟ ⎜ 2 2 ⎟ ⎜ √ √ ⎟ ⎜ 2 ⎟. ⎜ 2 ⎜− 0⎟ ⎠ ⎝ 2 2 0 0 1 of the strain tensor in the frame (Ox x x ) are given The components Sij 1 2 3 by: Sij = aik ajl Skl . We obtain: = S31 = S32 = S12 = 0, S33

d41 E = 5 × 10−6 , 2 d41 E =− = −5 × 10−6 . 2

= S12 = S11 S22 = −S12

Exercise 15.6 ∞ m, with the ∞-order axis parallel to A uniaxial stress has symmetry group m the stress-producing force.

Chapter 20 – Solutions to the exercises

485

The polarization (with symmetry ∞m), if it exists, must be at least as sym∞ m. metric as the intersection of the crystal’s point group and of m ∞ 1. (a) The intersection of group 32 and of m (with the ∞ order axis m parallel to the 3-fold axis) is 32. No polarization can exist.

− mm

32

32

Figure 20.38

(b) The intersection is group 2, where the 2-fold axis is parallel to the uniaxial stress. This group is consistent with a polarization parallel to this 2-fold axis, and thus parallel to the applied stress.

P

32

Figure 20.39 (c) The intersection is again group 2, with the 2-fold axis perpendicular to the uniaxial stress. This group is consistent with a polarization parallel to the 2-fold axis, hence perpendicular to the applied stress.

32

P

Figure 20.40 (d) A shear stress T12 has symmetry group mmm, where two of the mirrors are at an angle of 45◦ to the axes Ox1 and Ox2 . The intersection of groups 32 and mmm is empty. A polarization can exist but, if it does, its direction cannot be predicted.

486

Symmetry and Physical Properties of Crystals

=

empty set

32

Figure 20.41 For ZnO, with point group 6mm: (a) Uniaxial stress parallel to Ox3 : the intersection of the symmetry groups of the crystal and of the stress is group 6mm. There can exist a polarization parallel to Ox3 .

− mm

6mm

6mm

Figure 20.42

6mm

(b) Uniaxial stress parallel to Ox1 : the intersection of the symmetry groups of the crystal and of the stress is group mm2. There can exist a polarization parallel to Ox3 .

2.

− mm

mm2

Figure 20.43 (c) The same result as in (b) is obtained for a uniaxial stress parallel to Ox2 .

Chapter 20 – Solutions to the exercises

487

Exercise 15.7 1.

The intersection of group ¯42m and of the group, mmm, of the shear stress in the conﬁguration of Figure 20.44a is group mm2. There can exist a polarization parallel to the 2-fold axis because mm2 is a subgroup of ∞m if the ∞-order axis is parallel to the 2-fold axis.

2.

The intersection of group ¯42m with the group mmm of the shear stress in the conﬁguration of Figure 20.44b leads to group 222, which is not a subgroup of ∞m. No polarization can exist.

(a)

=

=

– 42m

(b)

– 42m

Figure 20.44

20.14. Exercises for Chapter 16 Note: for clarity, the diﬀerence between ne and no is very much exaggerated in all ﬁgures. Exercise 16.1 The light ray is parallel to the normal to the index surface. For the ordinary ray, δ = 0. For the extraordinary ray, we draw the normal to the index surface at Pe , the intersection of the index surface and the wave vector starting at O. Let ϕ and θ be the angles of the normal to the index surface and the wavevector, respectively, with axis Ox2 .

488

Symmetry and Physical Properties of Crystals x3 no

Pe

k

Po

O

ne

x2

Figure 20.45 We have δ = ϕ−θ. The equation of the extraordinary index surface is given by: x22 x2 + 32 = 1. 2 ne no

The normal to this ellipsoid, at Pe (x2 , x3 ), has components:

2x2 2x3 , 2 n2e no

and

n2 n2 x3 n2e = e2 tan θ = v tan θ if we set v = e2 , 2 n o x2 no no tan ϕ − tan θ (v − 1) tan θ tan δ = tan(ϕ − θ) = = . 1 + tan ϕ tan θ 1 + v tan2 θ tan ϕ =

The maximum value of δ is obtained for: d(tan δ) (1 + tan2 θ)(v − 1) 1 − v tan2 θ = 0, = 2 2 dθ (1 + v tan θ) so that i)

(v − 1) = 0 → v = 1. This is the special trivial case where ne = no and δ = 0, the minimum value.

ii) 1 − v tan2 θ = 0 → tan2 θ = ne ≈ no .

1 n2 − n2o ne − no n2 ≈ if = o2 → tan δ = e v ne 2no ne ne

Numerically: for quartz, δ = 0.33◦ . Since no and ne are not very diﬀerent, the angle θ for which δ is maximal is not very diﬀerent from 45◦ . Exercise 16.2 The ordinary ray goes through the plate without being deviated. The extraordinary ray is parallel to the normal to the extraordinary index surface at Pe . The same approach as in the above exercise shows that the components of the normal to the index surface which are respectively parallel to Ox2 and Ox3 are 2x2 /n2e and 2x3 /n2o . Let ϕ and θ be the angles respectively enclosed with

Chapter 20 – Solutions to the exercises

489

axis Ox3 by the normal to the index surface and the wave-vector. tan ϕ = Since, at Pe , x3 = x2 , tan ϕ =

x2 n2o . n2e x3

n2o . n2e

Numerically: ϕ = 51.2◦ . The deviation δ between the ordinary and extraordinary rays is δ = ϕ − θ = 6.2◦ . In the plate, the extraordinary wave-vector is perpendicular to the plate (Descartes’ law at the entrance surface). At the exit of the plate, it remains normal to the plate. The shift Δ = e tan δ = 0.11 cm = 1.1 mm. x2 ne

P e no x3

Figure 20.46 Exercise 16.3 1.

At the entrance of the prism, the ordinary and extraordinary waves propagate with no deviation of either the wave-vector or the ray direction. The ordinary ray is polarized perpendicular to the optic axis, hence parallel to the edge of the prism. δo and δe are the deviations of the ordinary and extraordinary rays respectively. The incidence angle i on the exit surface is equal to 30◦ for both waves. Let ro and re be the refraction angles for the ordinary and extraordinary waves respectively. In air, the directions of the wave-vector and of the ray coincide. The deviations δo and δe of the ordinary and extraordinary rays are δo = ro − i and δe = re − i. Hence: ro = δo + i = 56.02◦ and re = δe + i = 48.01◦ . Applying Descartes’ laws yields no = 1.6585 and ne = 1.4865.

2.

At the prism entrance, the ordinary and extraordinary wave-vectors are not deviated (application of Descartes’ laws to the wave-vectors). The same applies to the ordinary ray, but the extraordinary ray propagates along the normal at Pe to the index surface. The incidence angle of the ordinary and extraordinary wave-vectors on the exit surface is i = 30◦ ,

490

Symmetry and Physical Properties of Crystals C

A

x3

Ro

B 9

30°

Pe

i

Re

i

x2 e

30°

9

B

x3

re

Re Ro

Pe O

C

30°

A

(a)

x2

(b)

Figure 20.47 and the application of Descartes’ laws (to the wave-vectors) provides the direction of the wave-vectors in air at the prism exit. This is also the direction of the rays. For the ordinary ray, we ﬁnd ro = 56.02◦ , and the deviation, as above, is δo = 26.02◦ . For the extraordinary ray, we must determine the value n of the extraordinary index, equal to the radius vector of the index surface at Pe . The coordinates of Pe are x3 = n sin θ and x2 = n cos θ with θ = 30◦ . The following relation must hold: n2 cos2 θ n2 sin2 θ + =1 n2e n2o

so that

n2 = 1/

cos2 θ sin2 θ + n2e n2o

.

We ﬁnd n = 1.5245. Thus: n sin i = sin re so that re = 49.66◦ and δe = 19.66◦ . Exercise 16.4 The incident beam goes through the ﬁrst prism undeviated. At the exit from this prism, the calcite-air interface can give rise to total reﬂection. For the ordinary ray, total reﬂection occurs for an angle of incidence on the interface equal to the angle θ of the prisms, such that no sin θ > 1, so that θ > 37.09◦ . For the extraordinary ray, total reﬂection occurs for an angle θ such that ne sin θ > 1, so that θ > 42.29◦ . Thus, for an angle θ such that 37.09◦ < θ < 42.29◦ , the ordinary ray is totally reﬂected and the extraordinary ray is transmitted by the prism, with its polarization in the plane deﬁned by the optic axis and the wave-vector. The polarization is perpendicular to the plane of the ﬁgure.

Chapter 20 – Solutions to the exercises

491

9

9

9

De

9

Figure 20.48 Exercise 16.5 1.

In a uniaxial material, the electrical induction vector D of the ordinary wave is perpendicular to the optic axis, hence in this case in the plane of the ﬁgure. For the extraordinary wave, D is perpendicular to the plane of the ﬁgure. D

A glass 30°

9

Do

De 30°

re

9

i’o

B

Re

r’o

30°

9

r’e

Ro

calcite C

Figure 20.49 2.

In the calcite prism, propagation occurs as in an isotropic material with an index no for the ordinary wave and an index ne for the extraordinary wave. The angle of incidence for each of these waves at the calcite-glass interface is i = 30◦ . Applying Descartes’ laws to this interface yields: i)

for the ordinary wave, no sin i = n sin ro where n is the index of the glass. We obtain: ro = 32.34◦ .

ii) for the extraordinary wave, ne sin i = n sin re , and re = 28.65◦ . At the glass–air interface, the angles of incidence are respectively io = 2.34◦ and ie = 1.35◦ . Descartes’ laws yield, for the refraction angles: ro = 3.63◦ and re = 2.09◦ , respectively. The deviation between the two outgoing beams is α = ro + re = 5.72◦ .

492

Symmetry and Physical Properties of Crystals

Exercise 16.6 The ordinary ray goes through both prisms undeviated. In the ﬁrst prism, the wave-vector is parallel to the optic axis, and the index is no irrespective of the polarization. In the second prism, the index surface intersects the plane of the ﬁgure along two circles, with radii no and ne . The polarization of the ordinary ray is normal to the optic axis, and that of the extraordinary ray is perpendicular to the plane of the ﬁgure. For the latter polarization, the index is no in the ﬁrst prism, and ne in the second one. At the interface between the two prisms, the angle of incidence i is 30◦ and the refraction angle re is given by no sin i = ne sin re . We obtain re = 33.9◦ . The wave-vector and the ray are parallel. The angle of incidence on the exit surface is 3.9◦ and the angle of refraction is equal to the angle α we are seeking. ne sin 3.9◦ = sin α. Thus α = 5.8◦ . A

9

D

30° Do

9 i

re

Do

Do

9

De

9

De

Ro Re

30° B

C

Figure 20.50

20.15. Exercises for Chapter 17 Exercise 17.1 1.

For normal incidence, the wave-vectors and the rays for both the ordinary and the extraordinary waves go through the plate without being deviated. The polarization of the ordinary ray is perpendicular to the optic axis, and we choose this direction as the Oy axis. That of the extraordinary ray is parallel to the plane of the ﬁgure, and this will be the direction of axis Ox.

2.

The phase shift ϕ between a wave polarized parallel to Oy and a wave polarized parallel to Ox is given by: ϕ=

2π(no − ne )e . λ

Chapter 20 – Solutions to the exercises

493

9

O

x

9 Eo

z

Ee

z

Figure 20.51 Since the crystal is positive, ϕ is negative for all values of e. The wave is a quarter-wave plate if ϕ = − π2 (1 + 2p), with p a positive integer, so that: e=

λ (1 + 2p). 4(ne − no )

Numerically, e = 16.4 μm + p(32.8) μm. If e = 16.4 μm, ϕ = −π/2; if e = 49.2 μm, ϕ = −3π/2, which is equivalent to + π/2. For a half-wave plate, ϕ = −π(1 + 2p), so that: e=

λ (1 + 2p). 2(ne − no )

Numerically, e = 32.8 μm + p(65.6) μm. 3.

After the quarter-wave plate, the electric ﬁeld is, in Jones notation; √ 2 E Ex = 2 √ √ 2 2 Ey = E exp(iϕ) = − i E 2 2 for ϕ = − π/2 (e = 16.4 μm). After the plate, the wave is right-circular polarized. A left-circular polarization would be obtained by rotating the plate through π/2 around the incident beam. The phase shift would then be +π/2. Another approach consists in turning the polarizer by π/2 around the incident beam, so that the polarization is in the second quadrant.

4.

The second quarter-wave plate contributes an additional phase shift by −π/2, so that: √ √

2 2 1 1 π = E E , −1 −ie−i 2 2 2

494

Symmetry and Physical Properties of Crystals a wave with linear polarization parallel to the second bisector direction. This result is no surprise since the two quarter-wave plates together form a half-wave plate.

5.

Natural light is unpolarized, and it can be described as the sum of two components with perpendicular linear polarizations, with a phase shift that varies randomly in time. A quarter-wave plate contributes an additional phase shift by π/2 to each of these phase shifts, which vary randomly as before. After the plate, light therefore remains unpolarized.

Exercise 17.2 1.

The neutral lines are respectively parallel and perpendicular to the optic axis. In the case of quartz, the ordinary polarization (perpendicular to the optic axis) corresponds to the fast line, and the extraordinary polarization to the slow line (parallel to the optic axis). We choose axes Ox and Oy respectively parallel to the fast and slow neutral lines. y (ne) A P

j

i

x (no)

Figure 20.52 2.

After the polarizer (Fig. 20.52), the electric ﬁeld in Jones notation is:

E 0 cos α . E 0 sin α After the plate, it becomes:

E 0 cos α E 0 eiϕ sin α

,

2π where ϕ = (ne − no )e is the phase shift introduced by the plate. We λ can write: E = Eo (cos α i + eiϕ sin α j). After the analyzer (angle α with axis Oy), the amplitude E of the electric ﬁeld is given by: E = Eo cos α sin α(eiϕ − 1). The intensity I is proportional to: |E|2 = E × E ∗ = Eo2

sin2 2α iϕ (e − 1)(e−iϕ − 1) 4

Chapter 20 – Solutions to the exercises so that:

3.

495

I = I0 sin2 2α sin2

ϕ . 2

ϕ If α = 45◦ , then I = I0 sin2 . 2 i) I = 0 corresponds to a phase shift ϕ = 2pπ (p an integer), i.e. either no plate, or a plate with thickness such that the phase shift is a multiple of 2π. ii) I is maximum for ϕ = π(1 + 2p), i.e. a half-wave plate: e=

4.

λ (1 + 2p) 2(ne − n0 )

emin =

and

λ . 2(ne − n0 )

e = 0.2 mm. The extinguished wavelengths are such that: ϕ = 2pπ = (ne − n0 )e

2π λ

λ=

so that

(ne − n0 )e . p

For p < 3 and p > 5, the wavelengths are not all in the visible range. p = 3: λ = 0.667 μm,

p = 4: λ = 0.5 μm,

p = 5: λ = 0.4 μm.

Exercise 17.3 1.

The components of the electric ﬁeld after the plate are: Ex = E cos ωt Ey = E cos(ωt + ϕ). To determine the curve drawn out by the end of vector E as t varies, we eliminate time between the expressions of Ex and Ey . We have: cos ωt =

Ex E

and

sin ωt = −

Ey cos ωt cos ϕ Ex cos ϕ − Ey + = E sin ϕ sin ϕ E sin ϕ

so that:

Ex2 (Ex cos ϕ − Ey )2 + =1 E2 E 2 sin2 ϕ which is the equation of an ellipse. After the plate, the wave is therefore elliptically polarized. To determine the directions of the axes of the ellipse, we express the equation of the ellipse in an axis system (OXY Z) rotated by an angle θ with respect to the neutral lines of the plate, and we seek the value of θ such that, in this new frame, the coeﬃcient of the crossed term (EX EY ) be zero. The calculation yields θ = 45◦ , whatever the value of ϕ. This result is valid only because the incident polarization is at 45◦ to the neutral lines of the plate. The axes of the ellipse are at 45◦ to the neutral lines of the plate, hence respectively parallel and perpendicular to the direction of the incident vibration.

496

Symmetry and Physical Properties of Crystals √

2.

√ 2 2 (EX −EY ) and Ey = (EX +EY ), and the equation Ex = If θ = 2 2 of the ellipse takes the form: 45◦ :

2 EY2 EX = 1. + 2E 2 cos2 ϕ/2 2E 2 sin2 ϕ/2

The ratio

B ϕ B of the ellipse axes has the value: = tan . A A 2

Exercise 17.4 If we rotate the plate, between crossed polarizer and analyzer, around the incident beam, which is perpendicular to the plate, extinction will occur when the neutral lines of the plate are respectively parallel to the polarization directions of the polarizer and the analyzer. Exercise 17.5 1.

The ordinary ray is refracted under